Fundamentals of Radiation Materials Science
Gary S. Was
Fundamentals of Radiation Materials Science Metals and Alloy...

Author:
Gary S. Was

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Fundamentals of Radiation Materials Science

Gary S. Was

Fundamentals of Radiation Materials Science Metals and Alloys

With 381 Figures

123

Gary S. Was Nuclear Engineering and Radiological Sciences Materials Science and Engineering University of Michigan 1921 Cooley Bldg. 2355 Bonisteel Blvd. Ann Arbor, MI 48109-2104, USA e-mail: [email protected]

Library of Congress Control Number: 2007922926

ISBN 978-3-540-49471-3 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com c Springer-Verlag Berlin Heidelberg 2007 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting and production: LE-TEX Jelonek, Schmidt & V¨ockler GbR, Leipzig Cover design: eStudio Calamar S.L., F. Steinen-Broo, Girona, Spain Printed on acid-free paper

54/3180/YL – 5 4 3 2 1 0

This book is dedicated to my wife, LeeAnn

Preface

The purpose of this text is to provide a foundation for understanding the theory and mechanisms behind the effects of irradiation on metals and alloys. The subject is divided into three parts, each of which is subdivided into individual chapters that together, provide a unified picture of how radiation interacts with, and alters the structure and properties of metallic materials. Part I consists of three chapters and focuses on the radiation damage process and provides the formalism for the prediction of the amount and spatial configuration of the damage produced by bombarding particles. Chapter 1 treats the interactions between particles that result in the transfer of energy from the incident particle to the target atoms. Chapter 2 focuses on determination of the number of displacements produced by the bombarding particles, and Chap. 3 describes the spatial configurations of the resulting defects. While radiation damage describes the state of the irradiated material, radiation effects are concerned with defect behavior in the solid after formation. Part II (Chaps. 4–11) covers the physical effects of irradiation on metals. Chapter 4 provides background on the equilibrium concentration of point defects and their diffusion. Chapter 5 treats diffusion and reactions between point defects under irradiation that are fundamental to all of the observable effects. Chapter 6 describes radiation-induced segregation, which is a direct consequence of radiation-enhanced diffusion. Chapters 7 and 8 address the nucleation and growth of dislocation loops and voids, the defect aggregates that determine much of the behavior of irradiated alloys. Chapter 9 covers the stability of phases under irradiation and irradiationinduced precipitation and precipitate dissolution. Chapter 10 extends the effects of irradiation to the unique effects resulting from ion irradiation such as composition changes, sputtering, exfoliation, etc. Finally, Chap. 11 describes the application of ion irradiation to simulate the effects of neutron irradiation. Mechanical effects of radiation damage (Part III) are distinguished from physical effects by the application of stress. Hardening and deformation of alloys under irradiation are discussed in Chap. 12. The effect of irradiation on crack nucleation and propagation resulting either from static or fatigue loading is discussed in Chap. 13. Finally, creep deformation and growth are treated in Chap. 14. Irradiation also has a profound effect on corrosion and stress corrosion cracking and these degradation modes may prove to be limiting processes for many reactor designs. Chapter 15 combines the effects of irradiation with the processes of corrosion and stress corrosion cracking to examine how irradiation and the media can combine to degrade alloy behavior.

VIII

Preface

The chapters contain examples and illustrations of radiation effects and sample calculations to quantify and describe the observations. Problems at the end of each chapter are designed to reinforce the main concepts of each chapter and to challenge the reader on his or her comprehension of the topics covered within. Taken together, the chapter text, examples, illustrations and end-of-chapter problems provide a comprehensive treatment of the effects of irradiation on metals and alloys. The subject matter in this text will likely require two academic terms to complete. Many of the topics rely on a basic knowledge of disciplines that constitute the underlying basis for irradiation effects: thermodynamics and kinetics of solids, crystal structure, defects and dislocations, physical metallurgy, elasticity and plasticity, deformation and fracture and corrosion and stress corrosion cracking. The text either presents the requisite background for each of these topics, or provides references of other sources where good treatments can be found. This book should also be useful to researchers who would like to learn more about the subject, or who would like a more complete and integrated treatment of the topics than can be found in individual papers on the subject. While the chapters are integrated with one another and each chapter builds upon the sum of the previous chapters, it is possible to read selected chapters for just that topic. As a final comment, the author would like to note that this book was written by sorting, organizing and condensing information from several texts and numerous journal and conference papers in order to arrive at a comprehensive description of the processes constituting radiation materials science. A conscientious effort was made to acknowledge and give credit to the original sources of the ideas, theories, mathematical developments and drawings contained herein. For occasional oversights that may have occurred during the condensation process, the author offers his apologies. He is indebted to the many authors and publishers who provided material and illustrations for this text. Finally, the author wishes to acknowledge the many colleagues, students and friends who aided and advised him in this work. In particular, special thanks go to Jeremy Busby, Todd Allen, Michael Atzmon, Roger Stoller, Yuri Osetsky, Ian Robertson and Brian Wirth, for their substantive contributions to the content, to Elaine West, Brian Wagner and Sean Lemecha for their work on the illustrations, to Cherilyn Davis and Ovidiu Toader for their help in manuscript and movie preparation, to Lynn Rehn, Don Olander, Arthur Motta, Michael Nastasi, Steve Zinkle, K. Linga Murty, Lou Mansur and Peter Andresen for their chapter reviews, and to John King and Arden Bement for providing the inspiration to the author to pursue this field many years ago.

Ann Arbor, May 2007

Gary S. Was

Introduction

Radiation materials science describes the interaction of radiation with matter— a broad subject covering many forms of irradiation and of matter. Some of the most profound effects of irradiation on materials occur in the core of nuclear power reactors where atoms comprising the structural components are displaced numerous times over the course of their engineering lifetimes. The consequences of radiation to core components includes changes in shape and volume by tens of percent, increases in hardness by factors of five or more, severe reduction in ductility and increased embrittlement, and susceptibility to environmentally induced cracking. For these structures to fulfill their purpose, a firm understanding of the effect of radiation on materials is required in order to account for irradiation effects in design, to mitigate its effect by changing operating conditions, or to serve as a guide for creating new, more radiation-tolerant materials that can better serve their purpose. The attractiveness of nuclear power as a present day and future energy source is due to the vast improvements that have been made in the way reactors are operated and in our understanding of how these engineering systems degrade and fail. But the attractiveness of nuclear power is also driven by new concepts for advanced reactors that offer improvements in safety and reliability, radioactive waste production, energy efficiency and cost effectiveness. Nuclear power holds the promise for producing hydrogen in a clean and low cost process that would power a future hydrogen economy. Yet all of these improvements come at a cost. That cost is a greater demand on the materials used to build and operate these reactors. New concepts that promise better performance from this energy source also include more aggressive environments, higher temperatures and greater levels of irradiation. In his article in Nature, Butler [1] summarizes the challenges facing several promising advanced reactor concepts. In all but one, material behavior is the leading challenge in bridging the gap from concept to reality. The pivotal role of material behavior in the unique radiation environment created in a reactor core makes radiation materials science of paramount importance in the future of nuclear energy in the world. It is with this perspective that the objective of this text was formulated, to provide a sound, fundamental understanding of radiation effects in structural materials. Structural materials in reactor systems are predominantly crystalline, metallic alloys. Virtually all of the structural materials in reactors are metallic, and many of the materials proposed for the more aggressive conditions in advanced reactor concepts are metals as well. The types of radiation that can alter structural materials

X

Introduction

consist of neutrons, ions, electrons and gamma rays. All of these forms of radiation have the capability to displace atoms from their lattice sites, which is the fundamental process that drives the changes in structural metals described earlier. The inclusion of ions among the irradiating particles provides a tie-in to other fields and disciplines such as the use of accelerators for the transmutation of nuclear waste, or in the creation of new materials by ion implantation, ion beam mixing, plasma assisted ion implantation and ion beam assisted deposition. All of the concepts developed in this text for the interactions of ions with solids are applicable to these fields as well. The effect of irradiation on materials is rooted in the initial event in which an energetic projectile strikes a target. While the event is made up of several steps or processes, the primary result is the displacement of an atom from its lattice site. This book will address primarily crystalline solids in which the atom locations are defined by the crystalline structure. Irradiation displaces an atom from its site, leaving a vacant site behind (a vacancy) and the displaced atom eventually comes to rest in a location that is between lattice sites, becoming an interstitial atom. The vacancyinterstitial pair is central to radiation effects in crystalline solids and is known as a Frenkel pair (FP). The presence of the Frenkel pair and other consequences of irradiation damage determine the physical effects, and with the application of stress, the mechanical effects of irradiation. The radiation damage event, detailed in Chap. 1, is concluded when the displaced atom (also known as the primary knock-on atom, PKA) comes to rest in the lattice as an interstitial. This event consumes about 10−11 s. Subsequent events are classified as physical effects of irradiation. These effects include such phenomena as swelling, growth, phase change, segregation, etc. For example, it is possible to take a block of pure nickel, 1 cm on a side, irradiate it in a reactor (to a fluence of say, 1022 n/cm2 ) and measure it to be 1.06 cm on a side, representing a volume change of 20%! The volume change, or swelling, is isotropic and is due to the formation of voids in the solid (see for example, Fig. 8.1). Another example is irradiation growth. One can irradiate a cylindrical rod of uranium, 10 cm in length and 1 cm in diameter (7.85 cm3 ) to a fluence of ∼1020 n/cm2 and measure it to be 30 cm in length and 0.58 cm in diameter. The volume is unchanged (7.85 cm3 ), but the shape is highly distorted. Distortion at constant volume under irradiation is referred to as growth. Phase changes under irradiation are also common. A Ni–12.8at%Al, solid solution alloy irradiated with 5 MeV Ni+ ions to 1016 cm−2 will result in the formation of a Ni3 Al phase, which is separate and distinct from the parent phase (see for example, Fig. 9.3). The formation of a new phase is known as irradiation-induced phase formation and is of great significance in both ion and neutron irradiations. A last example of physical changes of irradiation is segregation. If a Ni–1at%Si alloy is bombarded with Ni+ ions at 525 ◦C and to a dose of one displacement per atom, the result is an enrichment of Si on the surface and at grain boundaries to values that are 20 to 60 times the amount in the bulk (see for example, Fig. 6.5). This redistribution of alloying elements to specific sites in the microstructure is

Introduction

XI

known as radiation-induced segregation and occurs in many alloys to a significant extent when irradiated at high temperatures. Irradiation-induced physical changes can indeed be dramatic. But how do they alter the structural integrity of components? This is the realm of mechanical effects of irradiation. Mechanical effects manifest themselves only under the application of a stress. The result is that alloys behave much differently than their unirradiated counterparts. For example, the impact energy of an irradiated steel can be drastically reduced. For unirradiated steels, the energy absorbed is a strong function of temperature, where at low temperatures, little energy is absorbed and the steel becomes very brittle, but with increasing temperature, the energy absorbing capacity of the steel increases dramatically. Irradiation of a steel with neutrons can cause a marked reduction in the strain and a several-fold increase in the strength of the steel. The result is an increase in strength by a factor of five and a decrease in ductility by over a factor of ten. Irradiation can also influence the way in which materials deform at high temperature. Under a constant load, there is almost a complete loss of creep strength due to severe embrittlement arising from irradiation. Finally, irradiation to a neutron fluence of >5 × 1020 n/cm2 (E > 1 MeV) results in accelerated intergranular cracking of iron- and nickel-base austenitic alloys in light water reactors. This cracking phenomenon is very pervasive in that it affects most all austenitic alloys in all types of water reactors. Clearly, any of these effects will have profound consequences on reactor component integrity. Understanding how they work is the key to designing around their detrimental effects or to developing new alloys that are more radiation tolerant. As it turns out, almost all of these effects have a common link: defects such as isolated vacancies and interstitials, clusters of vacancies and interstitials, dislocation loops and lines and voids and bubbles. The reader should keep these defect types in mind as we move from the radiation damage event through the physical effects to the mechanical effects. We will address the radiation damage event first as this is the basis for understanding all effects of irradiation. We will start by quantifying the extent of radiation damage and develop a physical description of the interaction process. In quantifying the displacement process, what we are seeking is a quantitative description of the number of vacancies and interstitials produced by an incoming projectile. Unless we can do this, we have no hope of understanding the extent of the damage. The importance of determining the effect of irradiation in terms of the production of defects is discussed in Chaps. 2 and 3, and is shown here with a simple illustration. The number of displacements created by a neutron flux is a complicated function of the energy dependence of that flux. Note in the top graph in Fig. I.1 that the dependence of the yield strength of a 316 stainless steel alloy on the neutron fluence is highly dependent on the particular neutron flux spectrum [2]. OWR is a test reactor with a typical LWR neutron spectrum, RTNS-II produced a pure 14 MeV source of neutrons and LASREF had a broad spectrum of high neutron energies. However, if the yield strength is plotted as a function of the displacement damage in the alloy (dpa = displacements per atom in the solid), then data from all three neutron sources collapses beautifully onto a single trend line (bottom graph in Fig. I.1) that

XII

Introduction

Fig. I.1. Comparison of yield stress change in 316 stainless steel irradiated in three facilities with very different neutron energy flux spectra. While there is little correlation in terms of neutron fluence, the yield stress changes correlate well against displacements per atom, dpa (after [2])

References

XIII

is independent of the flux spectrum. The independence of the yield strength-dpa correlation on the neutron spectrum indicates that dpa is a better representation of the effect of irradiation on materials properties than is the fluence, giving rise to our first objective. That is the determination of the quantity R, the number of displacements per unit volume per unit time: #displacements =N R≡ cm3 s

Eˆ Eˇ

φ (Ei )σD (Ei ) dEi ,

(I.1)

where N is the atom number density, Eˆ is the maximum energy of the incoming particle, Eˇ is the minimum energy of the incoming particle, φ (Ei ) is the energy dependent particle flux, and σD (Ei ) is the energy dependent displacement cross section:

σD (Ei ) =

Tˆ Tˇ

σ (Ei )ν (T ) dT ,

(I.2)

where Tˆ is the maximum energy transferred in a collision of a particle of energy Ei and a lattice atom, Tˇ is the minimum energy transferred in a collision of a particle of energy Ei and a lattice atom, σ (Ei , T ) is the cross section for the collision of a particle of energy Ei that results in a transfer of energy T to the struck atom, ν (T ) is the number of displacements per primary knock-on atom. So, ultimately, we want to determine: R=N

Eˆ Tˆ Eˇ

Tˇ

φ (Ei )σ (Ei , T )ν (T ) dT dEi .

(I.3)

The two key variables in this equation are σ (Ei , T ) and ν (T ). The term σ (Ei , T ) describes the transfer of energy from the incoming particle to the first atom it encounters in the target, the primary knock-on atom (PKA). Determination of this quantity is the goal of Chap. 1. The second quantity is ν (T ), the total number of displacements that the PKA goes on to make in the solid, and its determination is described in detail in Chap. 2. Taken together, they describe the total number of displacements caused by an incoming particle of energy Ei , and Eq. (I.3) accounts for the energy distribution of the incoming particles. The result is the total number of displacements in the target from a flux of particles with a known energy distribution. We will return to this equation often, as it is the essence of the quantification of radiation damage in solids.

References 1. Butler D (2004) Nuclear Power’s New Dawn. Nature 429:238–240 2. Greenwood LR (1994) J Nucl Mater 216:29–44

Contents

Movies accompanying the text are located at: www.sitemaker.umich.edu/was.

Part I Radiation Damage 1

The Radiation Damage Event . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Neutron–Nucleus Interactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Elastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.2 Inelastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.3 (n, 2n) Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.4 (n, γ ) Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Interactions Between Ions and Atoms . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 Collision Kinematics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Ionization Collisions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 Energy Loss Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.2 Range Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2

The Displacement of Atoms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73 2.1 Elementary Displacement Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73 2.1.1 Displacement Probability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74 2.1.2 The Kinchin and Pease Model for Atom Displacements . . . 75 2.1.3 The Displacement Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78 2.1.4 The Electron Energy Loss Limit . . . . . . . . . . . . . . . . . . . . . . . 83 2.2 Modifications to the K–P Displacement Model . . . . . . . . . . . . . . . . . . 85 2.2.1 Consideration of Ed in the Energy Balance . . . . . . . . . . . . . . 85 2.2.2 Realistic Energy Transfer Cross Sections . . . . . . . . . . . . . . . 86 2.2.3 Energy Loss by Electronic Excitation . . . . . . . . . . . . . . . . . . 87 2.2.4 Effects of Crystallinity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 2.3 The Displacement Cross Section . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105 2.3.1 Elastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 2.3.2 Inelastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 2.3.3 (n, 2n) and (n, γ ) Displacements . . . . . . . . . . . . . . . . . . . . . . . 107 2.3.4 Modifications to the K–P Model and Total Displacement Cross Section . . . . . . . . . . . . . . . . . . 108

3 4 4 11 14 15 17 17 24 44 44 57 66 68 71

XVI

Contents

2.4 Displacement Rates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 109 2.5 Correlation of Property Changes and Irradiation Dose . . . . . . . . . . . . 113 2.6 Displacements from Charged Particle Irradiation . . . . . . . . . . . . . . . . 115 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 119 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 121 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 3

The Damage Cascade . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 3.1 Displacement Mean Free Path . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 3.2 Primary Recoil Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 126 3.3 Cascade Damage Energy and Cascade Volume . . . . . . . . . . . . . . . . . . 131 3.4 Computer Simulations of Radiation Damage . . . . . . . . . . . . . . . . . . . . 133 3.4.1 Binary Collision Approximation (BCA) Method . . . . . . . . . 133 3.4.2 Molecular Dynamics (MD) Method . . . . . . . . . . . . . . . . . . . . 136 3.4.3 Kinetic Monte Carlo (KMC) Method . . . . . . . . . . . . . . . . . . . 138 3.5 Stages of Cascade Development . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 140 3.6 Behavior of Defects within the Cascade . . . . . . . . . . . . . . . . . . . . . . . . 143 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 152 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 153 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 154

4

Point Defect Formation and Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . 155 4.1 Properties of Irradiation-Induced Defects . . . . . . . . . . . . . . . . . . . . . . . 155 4.1.1 Interstitials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 155 4.1.2 Multiple Interstitials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 160 4.1.3 Interstitial–Impurity Complexes . . . . . . . . . . . . . . . . . . . . . . . 161 4.1.4 Vacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 162 4.1.5 Multiple Vacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 162 4.1.6 Solute–Defect and Impurity–Defect Clusters . . . . . . . . . . . . 162 4.2 Thermodynamics of Point Defect Formation . . . . . . . . . . . . . . . . . . . . 164 4.3 Diffusion of Point Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167 4.3.1 Macroscopic Description of Diffusion . . . . . . . . . . . . . . . . . . 168 4.3.2 Mechanisms of Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169 4.3.3 Microscopic Description of Diffusion . . . . . . . . . . . . . . . . . . 172 4.3.4 Jump Frequency, Γ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 174 4.3.5 Jump Frequency, ω . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 176 4.3.6 Equations for D . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 177 4.4 Correlated Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 180 4.5 Diffusion in Multicomponent Systems . . . . . . . . . . . . . . . . . . . . . . . . . 182 4.6 Diffusion along High Diffusivity Paths . . . . . . . . . . . . . . . . . . . . . . . . . 184 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 187 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 188 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 190

Contents

5

XVII

Radiation-Enhanced and Diffusion Defect Reaction Rate Theory . . . 191 5.1 Point Defect Balance Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 192 5.1.1 Case 1: Low Temperature, Low Sink Density . . . . . . . . . . . . 194 5.1.2 Case 2: Low Temperature, Intermediate Sink Density . . . . . 196 5.1.3 Case 3: Low Temperature, High Sink Density . . . . . . . . . . . 197 5.1.4 Case 4: High Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . . . 199 5.1.5 Properties of the Point Defect Balance Equations . . . . . . . . . 201 5.1.6 Deficiencies of the Simple Point Defect Balance Model . . . 203 5.2 Radiation-Enhanced Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 203 5.3 Defect Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 206 5.3.1 Defect Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 209 5.3.2 Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 5.3.3 Loss to Sinks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 5.3.4 Sink Strengths . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4 Reaction Rate-Controlled Processes . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4.1 Defect–Void Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4.2 Defect–Dislocation Interaction . . . . . . . . . . . . . . . . . . . . . . . . 212 5.5 Diffusion-Limited Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 212 5.5.1 Defect–Void Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 213 5.5.2 Defect–Dislocation Reactions . . . . . . . . . . . . . . . . . . . . . . . . . 215 5.6 Mixed Rate Control . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 217 5.7 Defect–Grain Boundary Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . 218 5.8 Coherent Precipitates and Solutes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 219 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 222 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 223 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 227

Part II Physical Effects of Radiation Damage 6

Radiation-Induced Segregation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 231 6.1 Radiation-Induced Segregation in Concentrated Binary Alloys . . . . . 233 6.1.1 Solution to the Coupled Partial Differential Equations . . . . . 239 6.1.2 Interstitial Binding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 240 6.1.3 Solute Size Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 6.1.4 Effect of Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 242 6.1.5 Effect of Dose Rate . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 245 6.2 RIS in Ternary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 246 6.3 Effect of Local Composition Changes on RIS . . . . . . . . . . . . . . . . . . . 250 6.4 Effect of Solutes on RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 6.5 Examples of RIS in Austenitic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . 256 6.6 RIS in Ferritic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 259 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 263 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 264 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 265

XVIII

Contents

7

Dislocation Microstructure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 267 7.1 Dislocation Lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 267 7.1.1 Dislocation Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 270 7.1.2 Description of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . 274 7.1.3 Displacements, Strains and Stresses . . . . . . . . . . . . . . . . . . . . 276 7.1.4 Energy of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 280 7.1.5 Line Tension of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . 281 7.1.6 Forces on a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 283 7.1.7 Interactions Between Dislocations . . . . . . . . . . . . . . . . . . . . . 289 7.1.8 Extended Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 292 7.1.9 Kinks and Jogs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 294 7.2 Faulted Loops and Stacking Fault Tetrahedra . . . . . . . . . . . . . . . . . . . 294 7.3 Defect Clusters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 298 7.3.1 Fraction of Defects Forming Clusters . . . . . . . . . . . . . . . . . . 298 7.3.2 Types of Clusters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 300 7.3.3 Cluster Mobility . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 304 7.4 Extended Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 306 7.5 Effective Defect Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 311 7.6 Nucleation and Growth of Dislocation Loops . . . . . . . . . . . . . . . . . . . 313 7.6.1 Loop Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313 7.6.2 Clustering Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 319 7.6.3 Production Bias-Driven Cluster Nucleation . . . . . . . . . . . . . . 321 7.7 Dislocation Loop Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 325 7.8 Recovery . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 329 7.9 Evolution of the Interstitial Loop Microstructure . . . . . . . . . . . . . . . . 332 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 335 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 338 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 341

8

Irradiation-Induced Voids and Bubbles . . . . . . . . . . . . . . . . . . . . . . . . . 343 8.1 Void Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 343 8.1.1 Equilibrium Void Size Distribution . . . . . . . . . . . . . . . . . . . . 345 8.1.2 Void Nucleation Rate . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 348 8.1.3 Effect of Inert Gas . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 355 8.1.4 Void Nucleation with Production Bias . . . . . . . . . . . . . . . . . . 362 8.2 Void Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 365 8.2.1 Defect Absorption Rates and Concentrations at Sink Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 366 8.2.2 Point Defect Balances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 370 8.3 Void Growth Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 372 8.3.1 Temperature Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . 377 8.3.2 Dose Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 380 8.3.3 Role of Dislocations as Biased Sinks . . . . . . . . . . . . . . . . . . . 384 8.3.4 Dose Rate Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 385 8.3.5 Irradiation Variable Shifts . . . . . . . . . . . . . . . . . . . . . . . . . . . . 388

Contents

XIX

8.3.6 Stress Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 393 8.3.7 Effect of RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 397 8.3.8 Effect of Production Bias . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 399 8.3.9 Void Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 402 8.3.10 Effect of Microstructure and Composition . . . . . . . . . . . . . . 404 8.3.11 Effect of Reactor Operating History . . . . . . . . . . . . . . . . . . . . 409 8.4 Bubble Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 415 8.4.1 Bubble Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 415 8.4.2 Growth Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 418 8.4.3 Bubble Growth by Dislocation Loop Punching . . . . . . . . . . . 421 8.4.4 Bubble Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 422 8.4.5 Helium Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 423 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 423 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 427 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 430 9

Phase Stability Under Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 433 9.1 Radiation-Induced Segregation and Radiation-Induced Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . 433 9.2 Recoil Dissolution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 436 9.3 Radiation Disordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 445 9.4 Incoherent Precipitate Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 450 9.5 Coherent Precipitate Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 455 9.6 Metastable Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 460 9.6.1 Order–Disorder Transformations . . . . . . . . . . . . . . . . . . . . . . 461 9.6.2 Crystal Structure Transformations . . . . . . . . . . . . . . . . . . . . . 461 9.6.3 Quasicrystal Formation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 9.7 Amorphization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 9.7.1 Heat of Compound Formation and Crystal Structure Differences . . . . . . . . . . . . . . . . . . . . . . 464 9.7.2 Solubility Range of Compounds and Critical Defect Density . . . . . . . . . . . . . . . . . . . . . . . . . . . 467 9.7.3 Thermodynamics and Kinetics of Amorphization . . . . . . . . 470 9.8 Phase Stability in Reactor Core Component Alloys . . . . . . . . . . . . . . 480 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 484 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 487 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 488

10 Unique Effects of Ion Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 491 10.1 Ion Irradiation Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 491 10.2 Composition Changes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 494 10.2.1 Sputtering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 495 10.2.2 Gibbsian Adsorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 501 10.2.3 Recoil Implantation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 503 10.2.4 Cascade (Isotropic, Displacement) Mixing . . . . . . . . . . . . . . 506

XX

Contents

10.2.5 Combination of Processes Affecting Surface Compositional Changes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 518 10.2.6 Implant Re-Distribution During Ion Implantation . . . . . . . . 522 10.3 Other Effects of Ion Implantation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 525 10.3.1 Grain Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 525 10.3.2 Texture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527 10.3.3 Dislocation Microstructure . . . . . . . . . . . . . . . . . . . . . . . . . . . 528 10.4 High Dose Gas Loading: Blistering and Exfoilation . . . . . . . . . . . . . . 530 10.5 Solid Phases and Inert Gas Bubble Lattices . . . . . . . . . . . . . . . . . . . . . 535 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 537 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 540 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 543 11 Simulation of Neutron Irradiation Effects with Ions . . . . . . . . . . . . . . 545 11.1 Motivation for Using Ion Irradiation as a Surrogate for Neutron Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 545 11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation 547 11.3 Particle Type Dependence of RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 550 11.4 Advantages and Disadvantages of the Various Particle Types . . . . . . 557 11.4.1 Electrons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 558 11.4.2 Heavy Ions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 562 11.4.3 Protons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 564 11.5 Irradiation Parameters for Particle Irradiations . . . . . . . . . . . . . . . . . . 565 11.6 Emulation of Neutron Irradiation Damage with Proton Irradiation . . 567 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 574 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 575 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 576 Part III Mechanical Effects of Radiation Damage 12 Irradiation Hardening and Deformation . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1 Elastic and Plastic Deformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1.1 Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1.2 Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 587 12.1.3 Tension Test . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 589 12.1.4 Yield Strength . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 592 12.2 Irradiation Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 594 12.2.1 Source Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 595 12.2.2 Friction Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 597 12.2.3 Superposition of Hardening Mechanisms . . . . . . . . . . . . . . . 606 12.2.4 Hardening in Polycrystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 612 12.2.5 Saturation of Irradiation Hardening . . . . . . . . . . . . . . . . . . . . 613 12.2.6 Comparison of Measured and Predicted Hardening . . . . . . . 617 12.2.7 Radiation Anneal Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . 620

Contents

XXI

12.2.8 The Correlation Between Hardness and Yield Strength . . . . 622 12.3 Deformation in Irradiated Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 626 12.3.1 Deformation Mechanism Maps . . . . . . . . . . . . . . . . . . . . . . . . 630 12.3.2 Localized Deformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 632 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 636 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 638 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 640 13 Fracture and Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 643 13.1 Types of Fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 643 13.2 The Cohesive Strength of Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 644 13.3 Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 647 13.4 Fracture Mechanics Tests . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 653 13.5 Elastic-Plastic Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . 655 13.6 Brittle Fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 658 13.7 Irradiation-Induced Embrittlement in Ferritic Steels . . . . . . . . . . . . . 664 13.7.1 Notched Bar Impact Testing . . . . . . . . . . . . . . . . . . . . . . . . . . 664 13.7.2 DBTT and Reduction in the Upper Shelf Energy . . . . . . . . . 666 13.7.3 Master Curve Approach . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 669 13.7.4 Factors Affecting the Degree of Embrittlement . . . . . . . . . . . 673 13.7.5 Embrittlement of Ferritic-Martensitic Steels . . . . . . . . . . . . . 677 13.7.6 Annealing and Re-Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . 678 13.7.7 Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 679 13.8 Fracture and Fatigue of Austenitic Alloys at Low to Intermediate Temperatures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 685 13.8.1 Effect of Irradiation on Fracture Toughness . . . . . . . . . . . . . 686 13.8.2 Effect of Irradiation on Fatigue . . . . . . . . . . . . . . . . . . . . . . . . 689 13.9 High-Temperature Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 690 13.9.1 Grain Boundary Voids and Bubbles . . . . . . . . . . . . . . . . . . . . 692 13.9.2 Grain Boundary Sliding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 697 13.9.3 Grain Boundary Crack Growth . . . . . . . . . . . . . . . . . . . . . . . . 700 13.9.4 Fracture Mechanism Maps . . . . . . . . . . . . . . . . . . . . . . . . . . . 703 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 703 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 705 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 707 14 Irradiation Creep and Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 711 14.1 Thermal Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 712 14.1.1 Dislocation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 716 14.1.2 Diffusional Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 723 14.2 Irradiation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 725 14.2.1 Stress-Induced Preferential Nucleation of Loops (SIPN) . . . 726 14.2.2 Stress-Induced Preferential Absorption (SIPA) . . . . . . . . . . . 729 14.2.3 Climb and Glide due to Preferential Absorption (PAG) . . . . 731 14.2.4 Climb and Glide Driven by Dislocation Bias . . . . . . . . . . . . 733

XXII

Contents

14.2.5 Transient Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 734 14.2.6 Loop Unfaulting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 738 14.2.7 Recovery Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 739 14.2.8 Diffusional Creep: Why There is no Effect of Irradiation . . 740 14.2.9 Comparison of Theory with Creep Data . . . . . . . . . . . . . . . . 741 14.2.10 Irradiation-Modified Deformation Mechanism Map . . . . . . . 744 14.3 Irradiation Growth and Creep in Zirconium Alloys . . . . . . . . . . . . . . . 746 14.3.1 Microstructure of Irradiated Zirconium Alloys . . . . . . . . . . . 747 14.3.2 Irradiation Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 750 14.3.3 Irradiation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 753 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 758 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 760 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 762 15 Environmentally Assisted Cracking of Irradiated Metals and Alloys . 765 15.1 Stress Corrosion Cracking: A Tutorial . . . . . . . . . . . . . . . . . . . . . . . . . 768 15.1.1 SCC Tests . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 770 15.1.2 SCC Processes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 772 15.1.3 Metallurgical Condition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 774 15.1.4 Crack Initiation and Crack Propagation . . . . . . . . . . . . . . . . . 774 15.1.5 Mechanisms of Stress Corrosion Cracking . . . . . . . . . . . . . . 783 15.1.6 Predictive Model for Crack Propagation . . . . . . . . . . . . . . . . 786 15.1.7 Mechanical Fracture Models . . . . . . . . . . . . . . . . . . . . . . . . . . 788 15.1.8 Corrosion Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 790 15.1.9 Hydrogen Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 790 15.2 Effects of Irradiation on Water Chemistry . . . . . . . . . . . . . . . . . . . . . . 791 15.2.1 Radiolysis and its Effect on Corrosion Potential . . . . . . . . . . 791 15.2.2 Effect of Corrosion Potential on IASCC . . . . . . . . . . . . . . . . 794 15.3 Service and Laboratory Observations of Irradiation Effects on SCC . 797 15.3.1 Austenitic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 797 15.3.2 Ferritic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 802 15.4 Mechanisms of IASCC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 805 15.4.1 Grain Boundary Chromium Depletion . . . . . . . . . . . . . . . . . . 805 15.4.2 Irradiation Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 806 15.4.3 Deformation Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 807 15.4.4 Selective Internal Oxidation . . . . . . . . . . . . . . . . . . . . . . . . . . 809 15.4.5 Irradiation-Induced Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . 809 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 809 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 811 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 812 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 815

Part I

Radiation Damage

1 The Radiation Damage Event

The radiation damage event is defined as the transfer of energy from an incident projectile to the solid and the resulting distribution of target atoms after completion of the event. The radiation damage event is actually composed of several distinct processes. These processes and their order of occurrence are as follows: 1. The interaction of an energetic incident particle with a lattice atom 2. The transfer of kinetic energy to the lattice atom giving birth to a primary knockon atom (PKA) 3. The displacement of the atom from its lattice site 4. The passage of the displaced atom through the lattice and the accompanying creation of additional knock-on atoms 5. The production of a displacement cascade (collection of point defects created by the PKA) 6. The termination of the PKA as an interstitial The radiation damage event is concluded when the PKA comes to rest in the lattice as an interstitial. The result of a radiation damage event is the creation of a collection of point defects (vacancies and interstitials) and clusters of these defects in the crystal lattice. It is worth noting that this entire chain of events consumes only about 10−11 s (see Table 1.1). Subsequent events involving the migration of the point defects and defect clusters and additional clustering or dissolution of the clusters are classified as radiation damage effects. What we first need to know in order to understand and quantify radiation damage, is how to describe the interaction between a particle and a solid that produces displacements, and later on, how to quantify this process. The most simple model is one that approximates the event as colliding hard spheres with displacement occurring when the transferred energy is high enough to knock the struck atom off its lattice site. In addition to energy transfer by hard-sphere collisions, the moving atom loses energy by interactions with electrons, the Coulomb field of nearby atoms, the periodicity of the crystalline lattice, etc. The problem is reduced to the following. If we can describe the energy-dependent flux of the incident particle and the energy transfer cross sections (probabilities) for collisions between atoms, then we can quantify the PKA production in a differential energy range and utilize this to determine the number of displaced atoms. In this chapter, we will concentrate on quantifying the energy transferred between interacting bodies as well as describing the energy transfer cross section. We

4

1 The Radiation Damage Event

Table 1.1. Approximate time-scale for the production of defects in irradiated metals (from [1]) Time (s)

Event

Result

10−18

Energy transfer from the incident particle Displacement of lattice atoms by the PKA Energy dissipation, spontaneous recombination and clustering

Creation of a primary knock-on atom (PKA) Displacement cascade

10−13 10−11 > 10−8

Defect reactions by thermal migration

Stable Frenkel pairs (single interstitial atoms (SIA) and vacancies) and defect clusters SIA and vacancy recombination, clustering, trapping, defect emission

will begin with neutron–nucleus reactions since the neutrality of the neutron makes the interaction particularly straightforward. Following creation of the PKA, subsequent interactions occur between atoms, and the positive charge of the nucleus and the negative charge of the electron cloud become important in understanding how atoms interact. In fact, atom–atom interaction is the low-energy limit of ion–atom interactions that occur in reactor cores and via ion irradiation using accelerators over a wide energy range and can lead to the last type of interaction: ionization collisions.

1.1 Neutron–Nucleus Interactions 1.1.1 Elastic Scattering By virtue of their electrical neutrality, elastic collisions between neutrons and nuclei can be represented as colliding hard spheres. When neutrons pass through a solid, there is a finite probability that they will collide with a lattice atom, imparting a recoil energy to the struck atom. This probability is defined by the double differential scattering cross section (in energy and angle), σs (Ei , Ef , Ω ), where, Ei and Ef are the incident and final energies and Ω is the solid angle into which the neutron is scattered. We are often only interested in the scattering probability as a function of Ei and the scattering angle. The single differential scattering cross section is:

σs (Ei , Ω ) =

σs (Ei , Ef , Ω ) dEf .

(1.1)

The total scattering probability for neutrons of energy Ei is:

σs (Ei ) =

σs (Ei , Ω ) dΩ .

(1.2)

1.1 Neutron–Nucleus Interactions

5

In the study of irradiation effects, we are interested in the behavior of the struck atom. So we are seeking σs (Ei , T ); the energy transfer cross section, or the probability that a neutron of energy Ei elastically scattering against an atom of mass M, will impart a recoil energy T to the struck atom. But first it is necessary to find T in terms of the neutron energy and the scattering angle. To do this, let us consider the dynamics of binary elastic collisions in the center-of-mass and laboratory frames. Figure 1.1a shows the trajectories of a neutron and the target nucleus before and after scattering, as seen from both the laboratory reference system and the center-ofmass system. The easiest way to obtain a relationship between the incident neutron energy, scattering angle and transferred energy is to analyze the dynamics of the collision in the center-of-mass (CM) system. When the collision is viewed in the center-of-mass system, the recoiling particles appear to move away from each other in opposite directions. Momentum conservation along the axes of approach and departure yield: c m − VcM = 0 c m − Vc M = 0 ,

(1.3)

and conservation of kinetic energy requires that: 1 2 1 1 1 2 mc + MVc2 = m2 c + MVc . 2 2 2 2 Using Eq. (1.3) to eliminate c and c , we get: 2 2 M M 1 1 1 1 2 m m + M Vc = + M Vc2 . 2 m 2 2 m 2

(1.4)

(1.5)

Therefore, Vc = Vc , and hence, c = c .

(1.6)

Since the target nucleus is at rest in the lab system and moving to the left with speed Vc in the CM system, the CM system itself must be moving to the right relative to the lab system with the same speed, Vc . Thus, if we use VCM to denote the speed of the CM system relative to the laboratory system, the magnitudes of VCM and Vc are the same (but opposite in direction). This can be restated as follows: c = − VCM = − Vc , and using Eq. (1.3), we find that: m VCM = . M+m

(1.7)

(1.8)

Recall that we want to relate T , the energy transferred to the struck atom, to φ , the scattering angle in the CM system. Using vector addition we can relate the recoil

6

1 The Radiation Damage Event

Fig. 1.1. Vector velocities (a) in the laboratory and center-of-mass (CM) systems, and (b) composite diagram relating velocities in the two systems

target nucleus velocity in the lab system, V , to φ as shown in Fig. 1.1b, which is a composite of the interaction in the lab and CM systems shown in Fig. 1.1a. Using the law of cosines: 2 V2 = VCM + Vc2 − 2VCMVc cos φ ,

and re-writing the velocities in Eq. (1.9) in terms of energy gives: 2 m 2T 2Ei 2m 2 2 V = , VCM = , and Vc2 = 2 Em , M m m+M M

(1.9)

1.1 Neutron–Nucleus Interactions

and substituting these expressions into Eq. (1.9) gives: m m mM 1/2 E + Em − 2 cos φ , T= Ei Em 2 i M m+M (m + M) or T = η1 η2 Ei +

η1 1/2 Em − 2η1 Ei Em cos φ , η2

7

(1.10a)

(1.10b)

where η1 = m/(m + M) and η2 = M/(m + M). Since we want to find the energy transferred, T as a function of initial energy to eliminate and scattering angle only, we use the relationship between Ei and Em Em . From Eqs. (1.7) and (1.8), we know that: m M c = − = . (1.11) m+M m+M Writing Eq. (1.11) in terms of energy gives: 2 M = Ei = η22 Ei . Em m+M

(1.12)

Substituting into Eq. (1.10b) and simplifying gives:

γ T = Ei (1 − cos φ ) , 2 where we define 4mM 4A γ= = , 2 (M + m) (1 + A)2

(1.13)

(1.14)

where 1 = m and A = M. Hence, T depends upon only one unknown, φ . Note the angular dependence of T on φ as shown in Fig. 1.2. The energy transferred rises from 0 at φ = 0 to a maximum of γ Ei at φ = π , or Tmin = Tˇ = 0 and Tmax = Tˆ = 0. That is, the energy transferred is a maximum when the particle backscatters and is a minimum when it misses the target, resulting in no change in course (φ = 0).

Example 1.1. For a neutron incident on a hydrogen atom, Tˆn-H /Ei = 1.0. But for a neutron incident on a uranium atom, Tˆn-U /Ei = 0.017. Conversely, comparing the interaction of an iron atom with 100 keV Xe+ ions or electrons, the value of γ for the Xe–Fe interaction is 0.83, yielding a Tˆ of 83,000 eV. However, the value of γ for e− –Fe interaction is 0.00004, giving a Tˆ of only 4 eV, which, as we will see in Chap. 2, is not enough to displace an iron atom from its lattice site. The scattering angles in the lab system for the incident particle (θ ) and the struck atom (α ) can be written in terms of the scattering angle in the center-

8

1 The Radiation Damage Event

Fig. 1.2. Energy transfer as a function of center-of-mass scattering angle

of-mass system (φ ) using the vector diagram in Fig. 1.1b. Applying the law of sines to Fig. 1.1b for the scattered particle: = c , sin(π − θ ) sin θ where c is given by Eqs. (1.6) and (1.7): −1 , c = VCM VCM and using Eq. (1.8), we have: c = VCM

M . m

Applying the law of cosines to the same triangle gives: 2 2 2 = c + VCM − 2VCM c cos(π − φ ) ,

and combining the last three equations to express θ as a function of φ yields: tan θ =

(M/m) sin φ . 1 + (M/m) cos φ

1.1 Neutron–Nucleus Interactions

9

Fig. 1.3. Scattering into the solid angular element dΩ defined by dA/r2

Applying the law of sines to the vector diagram in Fig. 1.1b for the struck atom gives: V Vc = , sin α sin φ and combining this result with Eqs. (1.6) and (1.9) where the energies are written in terms of velocities gives: tan α =

sin φ . 1 − cos φ

We are still interested in obtaining the probability that a given T will be imparted to the recoil atom. This depends on the differential cross section. We define σs (Ei , φ ) dΩ as the probability of a collision that scatters the incident particle into a center-of-mass angle in the range (φ , dΩ ) where dΩ is an element of solid angle about the scattering direction φ . Since differential probabilities written in transformed variables are equivalent, σs (Ei , φ ) can be written in terms of CM variables:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ .

(1.15)

Using Fig. 1.3 to relate dΩ to dφ , we have by definition: dΩ = dA/r2 ,

(1.16)

and from Fig. 1.4, we have: dΩ =

r dφ (2π r sin φ ) = 2π sin φ dφ . r2

(1.17)

Substituting Eq. (1.17) into Eq. (1.15) yields:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ = 2πσs (Ei , φ ) sin φ dφ .

(1.18)

10

1 The Radiation Damage Event Fig. 1.4. The solid angle dΩ subtended at the scattering angle φ by the incremental angle dφ

And since T = γ2 Ei (1 − cos φ ) then dT = 2γ Ei sin φ dφ , then we have:

σs (Ei , T ) =

4π σs (Ei , φ ) . γ Ei

(1.19)

Figure 1.5 shows the difference in the differential scattering cross section in units of area per unit solid angle vs. area per unit angle as in Eq. (1.18). Although the number of atoms scattered through an angle increment dφ about φ = π /2 is greater than that through an angular increment dφ about φ = 0 or π (Fig. 1.5a), the number intercepting the spherical surface per unit of solid angle is constant over all angles, φ (Fig. 1.5b). Hence dT / dφ varies in a sinusoidal manner with φ but dT / dΩ is independent of φ . Using Eqs. (1.2) and (1.18), the total elastic scattering cross section is:

σs (Ei ) =

σs (Ei , φ ) dΩ = 2π

σs (Ei , φ ) sin φ dφ .

Fig. 1.5. Isotropic differential scattering cross sections in units of (a) area per unit scattering angle and (b) area per unit solid angle

1.1 Neutron–Nucleus Interactions

11

If we assume that elastic scattering in the CM system is independent of scattering angle (i.e., scattering is isotropic), Fig. 1.6, then:

σs (Ei ) =

σs (Ei , φ ) dΩ = 2πσs (Ei , φ )

sin φ dφ = 4πσs (Ei , φ )

(1.20)

and

σs (Ei , T ) =

σs (Ei ) , γ Ei

(1.21)

which is independent of T ! That is, σs (Ei , T ), the probability that a neutron of energy Ei , elastically scattering against an atom of mass M, will impart a recoil energy T to the struck atom does not depend on the recoil energy. Now the average recoil energy can be calculated: Tˆ

Tˆ γ Ei Tˇ + Tˆ ˇ T σs (Ei , T ) dT T¯ = T ˆ ≈ = . = T 2 2 2 Tˇ σs (Ei , T ) dT

(1.22)

Applying Eq. (1.22) to the case of a 1 MeV neutron incident on elements of varying mass, we have the following: 1 MeV n on C: γ = 0.28 1 MeV n on Fe: γ = 0.069 1 MeV n on U: γ = 0.017

T¯ = 0.14 MeV T¯ = 0.035 MeV T¯ = 0.009 MeV

In addition to the elastic scattering just discussed, we can have energy transfer by inelastic scattering, (n, 2n) reactions and (n, γ ) reactions. The first two reactions become important above neutron energies of about 1.0 and 8.0 MeV, respectively, while the latter occurs at thermal neutron energies in 235 U. 1.1.2 Inelastic Scattering Inelastic scattering is characterized by a reaction in which the emitted particle is experimentally the same as the captured particle, but there is a loss of kinetic energy in the system. The energy is found in the excitation energy of the product nucleus, ∗ ∗ e.g., N14 (p, p’)N14 or C14 (n, n’)C14 . The differences in the energies of groups of scattered particles correspond to the energy separations of excited levels in the product nucleus: Q = ∑ KE f − ∑ KEi = ∑ M f c2 − ∑ Mi c2 . f

i

f

i

In an inelastic collision, a neutron is absorbed by the nucleus, forming a compound nucleus, which emits a neutron and a γ -ray. There may be more than one γ emitted and the nucleus may remain in an excited state during the course of an interaction. The inelastic scattering cross section can be divided into resolved and unresolved

12

1 The Radiation Damage Event

Fig. 1.6. Differential elastic scattering cross sections for C12 at 0.5 MeV and 14 MeV neutrons as a function of the cosine of the center-of-mass scattering angle (from [2])

resonance components [3]. For a given resonance ( jth resonance) of the target nucleus, the scattering cross section will be a function of Q j , the γ decay energy of the residual nucleus that is always negative. Analogous to Eq. (1.15) we can write differential equalities σs j (Ei , Q j , T ) dT = σs j (Ei , Q j , φ ) dΩ , so that:

σs j (Ei , Q j , T ) = σs j (Ei , Q j , φ ) 2π sin φ

dφ . dT

(1.23)

However, the expression for T in Eq. (1.13) is not valid for inelastic collisions since kinetic energy is not conserved. Instead we focus on the conservation of total energy. If the target nucleus M is at rest in the lab system and the particle m has energy Ei , then the energy balance in CM coordinates is: M Ei + Q j = Em + EM , M+m

(1.24)

and EM are the kinetic energies in CM where Q j is the reaction energy and Em coordinates of the exit particle and nucleus, respectively. In order that momentum is conserved: = MEM , mEm

(1.25)

and combining Eq. (1.24) with Eq. (1.25) (assuming that the masses of the projectile and target are unchanged after the reaction), yields: M M Ei Em = Qj + M+m M+m

1.1 Neutron–Nucleus Interactions

13

or Em = η2 (Q j + η2 Ei ) .

(1.26)

Recalling the general expression for T , Eq. (1.10b): T = η1 η2 Ei +

η1 172 E − 2η1 Ei Em cos φ , η2 m

from Eq. (1.26) yields and substituting in for Em

Qj γ γ A + 1 1/2 T (Ei , Q j , φ ) = Ei − . cos φ + Ei Ei + Q j 2 2 A A+1

(1.27)

Now, the expression for dT / dφ becomes:

Q j A + 1 1/2 dT (Ei , Q j , φ ) γ = Ei 1 + sin φ . dφ 2 Ei A

(1.28)

Note that in the case of elastic collisions, Q j = 0 and Eq. (1.27) reduces to Eq. (1.13). If we now assume that inelastic scattering is isotropic in the CM system, then we have:

σs j (Ei , Q j ) =

σs j (Ei , Q j , φ ) dΩ = 4πσs j (Ei , Q j , φ ) .

(1.29)

Substituting Eqs. (1.28) and (1.29) into (1.23) yields:

σs j (Ei , Q j , T ) =

σs j (Ei , Q j ) . Q j A + 1 1/2 γ Ei 1 + Ei A

(1.30)

for inelastic collisions in the resolved resonance region. When the compound nucleus is excited to high enough energies, the resonance levels overlap and are no longer individually distinguishable. The inelastic scattering cross section is treated as a continuum and is described by an evaporation model [3] with: ) f (Ei , Em σis Ei , Em , T = σis (Ei ) , and 1 1/2 Ei Em 4 A+1 E max ) m f (Ei , Em σis (Ei , T ) = σis (Ei ) dEm , (1.31) 1 1/2 0 Ei Em 4 A+1 ) is a distribution function for the energy E of the scattered neutron where f (Ei , Em m in the CM system that represents the probability that a neutron is evaporated from the moving compound nucleus, whose value in the CM system is a Maxwellian of

14

1 The Radiation Damage Event

nuclear temperature ED = kT : E f Ei , Em = m e(−Em /ED ) , I (Ei ) and

I (Ei ) = ED2

(1.32)

max max /E Em −Em D 1− 1+ e , ED

(1.33)

is a normalization factor such that E max m 0

dEm = 1 . f Ei , Em

(1.34)

is given by Eq. (1.26) with Q = Q , the lowest energy The maximum value of Em 1 is zero. level, and the minimum value of Em

1.1.3 (n, 2n) Reactions Reactions such as the (n, 2n) reaction are important in radiation effects since they produce additional neutrons that can either cause damage or transmutation reactions in components of interest. Following the 2n model, which is based on work by Odette [4] and Segev [5], a second neutron can only be emitted if the residual excitation of the nucleus after emission of the first neutron exceeds the binding energy of a neutron in the mass-M nuclide. The recoil energy after emission of the first neutron is taken to be the average value (cos φ = 0 in Eq. (1.10b)) and is shown in Fig. 1.7a in the lab system. We next analyze the second reaction (emission) in the CM system described in Fig. 1.7b. We begin by using the law of cosines to relate Vc to φ : V2 = V2 + Vc2 − 2VVc cos φ .

(1.35)

From Fig. 1.7a, we have: 1 MV 2 = T¯ 2

or V2 =

2T¯ , M

and from Fig. 1.7b we have: 1 (M − m)Vc2 = EM 2

or Vc2 =

2EM . M−m

Conservation of momentum requires: (M − m)Vc = mc ,

(1.36)

1.1 Neutron–Nucleus Interactions

15

and squaring gives: Vc2

=

m M−m

2

2 c =

2m E . (M − m)2 m

(1.37)

Substituting into the law of cosines, Eq. (1.35), gives: V2 =

2m 2m 2 ¯ 1/2 2T¯ + E T E − 2 cos φ , M (M − m)2 m (M − m)2 M m

(1.38)

is the mean recoil energy after emission of the where T¯ = η1 η2 Ei + (η1 /η2 ) Em 2 first neutron. Writing V in terms of energy gives the recoil energy following the second emission: 1 T = (M − m)V2 2 m 1/2 M−m ¯ m ¯ 1/2 Em = −2 (Em T ) cos φ T + M M−m M 1/2 1 A−1 ¯ 1 1/2 E − 2 T¯ Em = cos φ T + A A−1 m A 1/2 η1 A η1 A − 1 ¯ 1/2 T − 2 T¯ Em = Em + cos φ . (1.39) A − 1 η2 A η2

The (n, 2n) reaction cross section is a special case of the inelastic scattering cross section given in Eq. (1.31): σn,2n Ei , Em , Em , T = σn,2n (Ei )

σn,2n (Ei , T ) =

Em Em e−Em /ED e−Em /ED , I (Ei ) I (Ei , Em )

Ei −U Ei −U−E m Em e−Em /ED 0

I (Ei )

0

and

Em e−Em /ED dEm dEm , I (Ei , Em )

(1.40) max = E − U and I (E , E ) is Eq. (1.33) where I (Ei ) is given in Eq. (1.33) with Em i i m max max , and for (n, 2n) reactions, U = 0 [3]. with Em replaced by Em = Ei − U − Em

1.1.4 (n, γ ) Reactions Another class of reactions that can affect the extent of radiation damage involves photon emission. This reaction is important since the energy of the recoiling nucleus is sufficient to displace an atom. As we will see later, this type of displacement is particularly important in radiation damage in reactor pressure vessels in which the gamma flux is more comparable to the fast neutron flux than in the reactor core. Recalling the momentum and energy conservation laws of Eqs. (1.3) and (1.4) and

16

1 The Radiation Damage Event

Fig. 1.7. Vector velocities for the (n, 2n) reaction in (a) the lab system and (b) the center-ofmass system

Fig. 1.1, which for (n, γ ) reactions, Ei ∼ 0 (since these reactions occur with thermal neutrons of energy 0.025 eV), Ef ≡ 0 (since there is no scattered neutron) and Q is the equivalent of the mass difference between the initial particles and the compound nucleus. When the compound nucleus (CN) de-excites, it emits a γ -ray with this energy. Conservation of momentum says that the nucleus must recoil with momentum: (m + M)Vc =

Eγ . c

(1.41)

Note that this is an approximation since we have not subtracted the mass defect from the compound nucleus. Squaring both sides of Eq. (1.41) and dividing by 2(m + M) gives: Eγ2 1 (m + M)Vc2 = . 2 2(m + M)c2 As in the case of elastic scattering, T is given by: 2 M+m 2 T = VCM + Vc − 2VCMVc cos φ , 2 but VCM Vc so to a good estimate: Eγ2 m+M 2 T∼ = . V = c 2 2(M + m)c2 We will assume further that this value of T represents the maximum recoil energy. But since not all of Q will be emitted in a single γ -ray, we approximate the average recoil energy as half the value of the maximum recoil energy, giving: T¯ ∼ =

Eγ2 . 4(M + m)c2

(1.42)

1.2 Interactions Between Ions and Atoms

17

The radiative capture cross section is derived from the Breit–Wigner single-level formula when the target nucleus has zero intrinsic angular momentum and the compound nucleus has a neutron width Γn and a radiation width Γg , and a total width Γ , and E0 is the resonance energy and λ is the wavelength [6]:

σn,γ (Ei ) = πλ 2

ΓnΓγ . (Ei − E0 )2 + (Γ /2)2

(1.43)

Expressing Eq. (1.43) in terms of σ0 , the maximum value of the radiative cap√ ture cross section (at E = E0 ) and taking the Γn proportional to 1/λ and to E gives: E0 1 . (1.44) σn,γ (Ei ) = σ0 Ei [(Ei − E0 ) /(Γ /2)]2 + 1 Table 1.2 provides a summary of the energy transfer and the energy transfer cross sections for the various types of reactions covered in Sect. 1.1.

1.2 Interactions Between Ions and Atoms Ion–atom or atom–atom collisions are governed by interactions between the electron clouds, the electron cloud and the nucleus, and between the nuclei. These interactions are described by what are known as interatomic potentials. In order to develop descriptions of energy transfer cross sections for interactions between atoms, we need descriptions of the potential function that governs that interaction. Unfortunately, there exists no single function that describes all interactions, but rather, the nature of the interaction is a strong function of the atom energies, and hence their distance of closest approach of their nuclei. The following section provides a summary of interatomic potentials adapted from Chadderton [7]. 1.2.1 Interatomic Potentials The end product of the neutron–nuclear interaction is the creation of the primary knock-on atom with some amount of kinetic energy. This atom will, of course, make subsequent collisions with other atoms in the solid. Knowledge of the forces acting between two colliding atoms represents the most fundamental aspect of radiation damage, without which a proper description of the primary event and the ensuing defect structure is impossible. Our interest lies in the forces between like atoms, unlike atoms, or ions and atoms. The description of interactions between atoms is done using potential functions. Recall that the atoms are (usually) electrically neutral but are composed of positive and negative components that do not cancel at all points in space. It is well known that the potential energy between two point

18

1 The Radiation Damage Event

Table 1.2. Energy transfer and energy transfer cross sections for various types of neutron– nuclear collisions Type of collision

Elastic scattering

Energy transfer and energy transfer cross section

γ T = Ei (1 − cos φ ) 2

(1.13)

σs (Ei ) γ Ei

(1.21)

σs (Ei , T ) = Inelastic scattering

Qj γ γ A + 1 1/2 cos φ + T (Ei , Q j , φ ) = Ei − E i E i + Qi 2 2 A A+1 resonance region

σs, j (Ei , Q j , T ) =

σs, j (Ei , Q j )

Qj l +A γ Ei 1 + Ei A unresolved resonance region

σn,2n (Ei , T ) =

E max m

Ei −U Em e−Em /ED I (Ei ) 0 Ei −U −E

×

(n, γ )

1/2

) f (Ei , Em dEm 1 0 1/2 4 EE A+1 i m 1/2 η1 A η1 A − 1 ¯ 1/2 T¯ Em T −2 T= E + cos φ A − 1 η2 m A η2

σis (Ei , T ) = σis (Ei )

(n, 2n)

Equation in text

m

0

Em −Em /ED dEm dEm )e I (Ei , Em

Eγ2 4(M + m)c2 1 E0 σn,γ (Ei ) = σ0 Ei [(Ei − E0 )/(Γ /2)]2 + 1 T¯ ∼ =

(1.27)

(1.30)

(1.31)

(1.39)

(1.40) (1.42) (1.44)

charges of the same sign separated by a distance r is described by the well know Coulomb equation: V (r) =

ε2 , r

(1.45)

where ε is a single unit charge. However, in the case of atoms, we have a charged nucleus surrounded by an electron cloud of opposite charge. It is evident that the potential function describing the interaction between atoms is far more complicated. Even in the simplest cases, V (r) has never been determined exactly, but some simple considerations show that it must be dominated by two distinct contributions over the

1.2 Interactions Between Ions and Atoms

19

range of separation in which we are interested. Perhaps the simplest of all potential functions is the “hard-sphere” approximation. This potential is described as follows: 0 for r > r0 V (r) = (1.46) ∞ for r < r0 . This potential function describes an interaction with an infinitely sharp cut-off at the atomic radius r0 . At distances greater than this radius the interaction vanishes, while at distances less than r0 the magnitude is infinity. This description is analogous to the behavior of billiard balls and hence, the atoms in this model are described as acting as such. Clearly this is not a very realistic description of atom–atom interaction since we know that the electron shells can overlap. Figure 1.8 shows how the interatomic potential actually varies with separation. At large separation, the principal interaction is supplied by the Coulomb forces while for smaller separations, the central field repulsive force is dominant. A similar relationship applies to all crystals regardless of the nature of binding. In all cases there is a smooth curve with a minimum at the separation distance corresponding to the nearest neighbor distance in the lattice, re (also referred to as D). In describing the interaction between atoms, we will use two yardsticks for points of reference. One is the Bohr radius of the hydrogen atom, a0 = 0.053 nm, which provides a measure of the position of the atomic shells. The other is re , the spacing between nearest neighbors in the crystal (typically ∼ 0.25 nm). When r re , electrons populate the lowest energy levels (closed shells) of the individual atoms and only the outer valence shells will have empty levels. As two atoms are brought together, the valence shells begin to overlap and weak attractive forces such as van de Waals forces may develop. When a0 < r ≤ re the closed inner shells begin to overlap. Since the Pauli exclusion principle demands that some electrons change their levels, and hence move to higher energy levels, the extra energy supplied in forcing the atoms together constitutes a positive potential energy of interaction. This is known as closed shell repulsion and the potential that most accurately describes

Fig. 1.8. Variation of interatomic potential with separation, r. Coulomb forces dominate at large separations (b) and the central repulsive force dominates at small separations (a), and at intermediate distances, there is a smooth transition between the two extremes with a minimum corresponding to the equilibrium separation distance, re or D

20

1 The Radiation Damage Event

this region is the Born–Mayer potential: V (r) = A exp(−r/B) ,

(1.47)

where A and B are constants determined from the elastic moduli [8]. Although this function was first used by Born and Mayer to represent core ion repulsion in their theory of ionic crystals, it is perfectly valid for separations on the order of the equilibrium separation, re , and is useful in treatments of threshold or near-threshold collisions where the impact parameter is of the order re . When r a0 , Coulomb interaction between the nuclei dominates all other terms in V (r): V (r) =

Z1 Z2 ε 2 . r

(1.48)

At slightly larger distances, the nuclear charges are electrostatically “screened” by the space charge of the innermost electron shells that have entered the internuclear space. The potential describing this behavior is known as the screened Coulomb potential [8, 9, 10, 11, 12]: Z1 Z2 ε 2 V (r) = exp(−r/a) , (1.49) r where a =

Ca0

2/3 2/3 1/2 Z1 + Z2

or a =

Ca0 (Z1 Z2 )1/6

, C = 0.8853 and a0 is the Bohr radius

of the hydrogen atom. More generally, screening by the electron cloud is described by a screening function, χ (r) that is defined as the ratio of the actual atomic potential at a radius r to the Coulomb potential. The function of χ (r) is to moderate the Coulomb potential to describe the interaction between atoms at all separation distances. For large distances, χ (r) will tend toward zero, and at very small distances, χ (r) will tend toward unity. This is one way in which a single interatomic potential function can be used to describe all collisions. We have now described two regimes of interaction. At small separations (r a0 ) the screened Coulomb term dominates all others, with the screening effect decaying exponentially with the separation distance. In the region a0 < r ≤ re electronic interaction dominates and is best described by the Born–Mayer potential. At intermediate separations there is no satisfactory description of the nature of atomic interaction. Unfortunately, it is exactly in this region where information is needed to provide a proper analytical description of radiation damage. Nevertheless, we may make a first approximation to the total potential by summing the controlling potentials at large and small separations: V (r) =

Z1 Z2 ε 2 exp(−r/a) + A exp(−r/B) , r

(1.50)

where A = 2.58 × 10−5(Z1 Z2 )11/4 eV, B = 1.5a0 /(Z1 Z2 )1/6 are empirical formulae suggested by Brinkman [11], consistent with observed compressibilities and elastic

1.2 Interactions Between Ions and Atoms

21

moduli in the noble metals Cu, Ag and Au. Unfortunately, there is a little experimental information about the forces between metal atoms, which is our primary interest. Figure 1.9 shows that the first term dominates for small separation and the second for large. Brinkman suggested a model for the interaction between two identical atoms in which the nucleus is surrounded by a rigid charge distribution ρε and it is assumed that both atoms supply a screened Coulomb field of the same type: V (r) =

r Z 2 ε 2 −r/a 1− e . r 2a

(1.51)

This relation approaches the Coulomb repulsion as r approaches zero and changes sign √ at r = 2a, becoming a weak attractive potential with a minimum at r = a(1 + 3). However, this potential predicts a strong interaction energy at large distances and may not represent the true physical picture for metals. Brinkman formulated a new potential function: V (r) =

AZ1 Z2 ε 2 exp(−Br) . 1 − exp(−Ar)

(1.52)

Note that for small values of r the potential closely approximates the Coulomb repulsive interaction, i.e., lim V (r) →

r→∞

Z1 Z2 ε 2 , r

Fig. 1.9. Behavior of various potential functions over a range of separation distances between copper atoms

22

1 The Radiation Damage Event

and at large separation, the potential equation approximates the exponential repulsion of the Born–Mayer type: lim V (r) → AZ1 Z2 ε 2 exp(−Br) .

r→∞

1/3

The constant B is defined as B = Zeff /Ca0 , where Zeff = (Z1 Z2 )1/2 , and C is of the order 1.0 or 1.5. The constant A depends on the compressibility and bulk modulus, which depend on the overlap of closed electron shells. An empirical expression for 0.95 × 10−6 7/6 Zeff . Substituting for A, B and C (= 1.5) into Eq. (1.52) gives: A is A = a0

1/3 exp −Zeff r/1.5a0 1/2

, V (r) = 1.9 × 10−6Zeff ER (1.53) 7/6 1 − exp −0.95 × 10−6Zeff r/a0 where ER = ε 2 /2a0 is the Rydberg energy (13.6 eV). It should be noted that although the potential is a reasonably reliable function for all metals whose atomic number exceeds 25 over the range r < 0.7re , it should not be used near r = re since in the derivation it has been implicitly assumed that all interatomic distances are close to those of Cu, Ag and Au. It is therefore not a valid potential to use in calculating formation and migration energies of point defects. Two other potentials should be discussed. The first is the Firsov or Thomas– Fermi two-center potential. This potential function is an improvement over the screened Coulomb potential by virtue of the fact it takes into account the change in electron energy connected with the mutual approach of the nuclei. The potential can be written as: V (r) =

χ (r) , r

where χ (r) is the screening function. In the case of the screened Coulomb potential:

χ (r) = χB (r) and χB (r) = Z1 Z2 ε 2 exp (−r/a) , while in the Firsov potential:

1/2 1/2 2/3 r χ (r) = χTF (r/a) = χ Z1 + Z2 , a

(1.54)

(1.55)

so that we have:

Z1 Z2 ε 2 1/2 1/2 2/3 r χ Z1 + Z2 V (r) = , r a

(1.56)

1.2 Interactions Between Ions and Atoms

23

where

1/2 1/2 2/3 r χ Z1 + Z2 a is a screening function. The second potential of interest is the Thomas–Fermi–Dirac two-center potential (TFD). The Thomas–Fermi–Dirac statistical model of the atom was employed to calculate a potential from first principles. As a consequence, this potential takes into account exchange effects and places a finite boundary, defined by rb , on the spatial distribution of the electron cloud density ρε . The potential obtained for like atoms is: Z 2 ε 2 1/3 r − α Z + Λ¯ , χ Z V¯ (r) = r a

(1.57)

ε where α ∼ = 3.16 × 10−3 and Λ¯ is a set of integrals over exact single-center eleca0 tron densities. Calculations using this potential have shown that for very small separations of less than ∼ 0.3a0, V¯ (r) agrees well with other theoretical curves and with experiment, while in the range ∼ 0.3a0 to 3a0, V (r) agrees with other theoretical and experiment results better than the screened Coulomb potential or the Firsov potential [7]. In selecting the appropriate potential for a specific collision problem, the range of separation can be determined by equating the available kinetic energy to the potential and hence obtaining the smallest separation. The important interaction terms for the calculated separation can then be determined. For interactions between metal atoms at low kinetic energies, 10−1 to 103 eV, the Born–Mayer term alone is sufficient with constants given in Eq. (1.50). In cases of atom–atom collisions in the collision cascade, where energies from 103 to 105 eV are involved, an inverse power potential is extremely convenient. Such a potential can be formulated by fitting a function C/rs to one of the above potential functions over a limited range of r. For example, one can fit an inverse square (s = 2) function to the screened Coulomb potential at r = a, obtaining the same slope, ordinate and curvature. This function is [13]: 2

V (r) =

Z1 Z2 ε 2 a −1 e . r2

(1.58)

For a limited range of r, this can be used as an approximate potential. Re-writing using the expression in Eq. (1.49) for a gives: V (r) =

a 2 2ER 0 (Z1 Z2 )5/6 . e r

(1.59)

24

1 The Radiation Damage Event

A convenient alternative for numerical calculations uses the fact that hence: a 2 0 V (r) = 10 (Z1 Z2 )5/6 eV . r

2ER ∼ = 10 eV, e (1.60)

This potential also applies to heavy ion bombardment in the energy range 103 to 105 eV. In the case of light ions at high energy, such as 5 MeV protons, the simple Coulomb potential is adequate. Table 1.3 summarizes the various potential functions and their regions of applicability. But how do we go about verifying a potential function? For example, how do we determine the constants A and B in the Born–Mayer potential for a specific element? Since the Born–Mayer potential is based on small displacements from equilibrium (i.e., re ), we can obtain these constants from bulk property measurement of the solid,e.g.,compressibility, elastic moduli, etc. If we expand the potential φ (r) 2 2φ dφ d φ d r + 1/2 r2 + · · · , then the coefficient of is the as φ0 + dr 0 dr2 0 dr2 0 curvature of the energy–distance curve at r = re shown in Fig. 1.8. How then do we know that a given potential does or does not properly describe the interaction in a region of r? We can make this determination by scattering measurements or by measuring the range of ions in solids. Since V (r) describes the nature of the interaction, it will also tell us about σs (Ei ), that can be determined by scattering experiments. Also, range measurements give a good indication of how many interactions must have occurred in order to place the ion in its deposited location. Both of these sets of experiments will provide information on the adequacy of the chosen potential function to accurately describe the interaction between atoms in the solid. With some appreciation for the way in which neutral atoms or atoms and ions interact, we are now prepared to describe a collision between these species, which is in some ways very similar to, and in other ways very different from neutron–nuclear collisions. The resulting formalism will provide us with the tools to determine the energy transferred from the incident atom to the struck atom along with the energy transfer cross section. The following treatment is adapted from Thompson [13]. 1.2.2 Collision Kinematics The orbits of two colliding atoms are shown in Fig. 1.10 relative to the center of mass of the masses M1 and M2 . Particle locations are most conveniently denoted in polar coordinates (r1 , ψ ) and (r2 , ψ ) for masses M1 andM2 , respectively. The impact parameter is b, ψ is the scattering angle of the struck atom in the lab system and φ is the asymptotic scattering angle when the interparticle spacing approaches infinity. The impact parameter is defined as the distance between the asymptotic trajectories of the colliding particles as shown in Fig. 1.10. We are interested in determining the detailed orbits by expressing φ is a function of b. This result will then be used to determine the scattering cross section.

Inverse square

TFD two-center

Firsov

Brinkman II

Brinkman I

r < 0.7re

A=

Z > 25

a 2 2Er 0 (Z1 Z2 )5/6 e r

a/2 < r < 5a

0.95 × 10−6

a0 /Z 1/3

ER = Rydberg energy = 13.6 eV

(1.59)

(1.57) cloud density vanishes

rb = Radius at which the electron

(1.52)

(1.56)

7/6

Zeff

χ is screening function

a0 1/3 B = Zeff /Ca0 C∼ = 1.5

a∼ =

r r0 ∞ for r < r0 V (r) = A exp(−r/B)

Hard-sphere

Born–Mayer

Definitions

Range of applicability

Equation for V (r) =

Potential

Table 1.3. Summary of potential functions

1.2 Interactions Between Ions and Atoms 25

26

1 The Radiation Damage Event

Fig. 1.10. Collision orbits in the center-of-mass system

The radial and transverse velocity of mass M1 are r˙1 and r1 ψ˙ in polar coordinates, and the resultant velocity is (˙r12 + r12 ψ˙ 2 )1/2 . The velocity components are the same for mass M2 with the subscript 2 substituted for 1. Conservation of energy requires that the total energy of any system remain constant. The energy in the lab 1 M1 reference system is just Ei = M1 2 = ET . Recall that VCM = , and that 2 M1 + M2 the kinetic energy of the center of mass itself (in the lab system) is: M1 1 2 = ECM = (M1 + M2 )VCM Ei . 2 M1 + M2 Hence, the energy in the CM system that is available for transformation is the total kinetic energy less the motion energy of the CM system: M2 . (1.61) E = ET − ECM = Ei − ECM = Ei M 1 + M2 In an elastic collision, the sum of the potential and kinetic energies at any point in the orbit must equal the asymptotic sum of kinetic energies, so: 1 M2 1 = M1 r˙12 + r12 ψ˙ 2 + M2 r˙22 + r22 ψ˙ 2 + V (r1 + r2 ). Ei M1 + M2 2 2 (1.62) asymptotic sum of kinetic energy at any point potential energy in orbit energy

1.2 Interactions Between Ions and Atoms

Letting r = r1 + r2 be the total separation distance, and r1 = M1 r, and the energy balance of Eq. (1.62) simplifies to: M1 + M2

27

M2 r, r2 = M1 + M2

1 η Ei = μ r˙2 + r2 ψ˙ 2 + V (r) , 2

(1.63)

M2 M1 M2 and μ = is the reduced mass. M1 + M2 M1 + M2 The law of conservation of angular momentum demands that the value at any point in the orbit must equal the asymptotic value. Recall that: M2 M1 and V2 = VCM = , = − VCM = M1 + M2 M1 + M2

where η =

so that the asymptotic value of the angular momentum is given by: M1 1 b1 + M2 2 b2 =

M1 M2 (b1 + b2 ) = μ b . M1 + M2

(1.64)

The angular momentum at any point is given by: 2 2 M2 M1 2 ˙ 2 ˙ M1 r1 ψ + M2 r2 ψ = M1 r + M2 r ψ˙ M1 + M2 M1 + M2 = μ r2 ψ˙ ,

(1.65)

hence:

μ r2 ψ˙ = μ b .

(1.66)

Substituting from Eq. (1.66) into Eq. (1.63) to eliminate ψ˙ and solving for r˙, we obtain: r˙ =

1/2

1/2 2 b2 η Ei 1 − 2 − V (r) . μ r

(1.67)

The algebra for this step is as follows. Multiplying out the terms of Eq. (1.63) gives: 1 1 2 b 2 η Ei − μ r˙2 = μ 2 + V (r) , 2 2 r and re-arranging gives: 1 2 b 2 1 η Ei − μ 2 = μ r˙2 + V (r) . 2 r 2

(1.68)

28

1 The Radiation Damage Event

Recall that Ei = 1/2M12 and therefore, 2 = 2Ei /M1 and we can eliminate so μ b 2 Ei that the second term on the left hand side of Eq. (1.68) becomes − . Since M1 r2 M1 M2 μ= and μ /M1 = η , then: M1 + M2 b2 μ r˙2 μ r˙2 b2 + V (r) , and η Ei 1 − 2 = + V (r) , η Ei − η Ei 2 = r 2 r 2 or r˙ =

1/2

1/2 2 b2 η Ei 1 − 2 − V (r) , μ r

which is the same as in Eq. (1.67). Note that r reaches the distance of closest approach when r˙ = 0. At this point: b2 V (r) = η Ei 1 − 2 , r

(1.69)

and Vmax = η Ei (at b = 0) which represents a “head-on” collision. So if a particle strikes a target atom of equal mass, then V max = 1/2Ei . 2 2 When r → ∞, V (r) → 0 and r˙ = η Ei , or r˙2 = 2Ei /M1 , Ei = 1/2M1r˙2 (and μ r˙ = at r → ∞), so Ei = 1/2M1 2 . Recall that we are looking for φ as a function of b. Going back to Eq. (1.67) and dividing r˙ in Eq. (1.67) by ψ˙ from Eq. (1.66) we have: 1/2

1/2 2 2 r dr r˙ b2 . = =− μ Ei 1 − 2 − V (r) ψ˙ dψ μ r b

(1.70)

The minus sign in front of the quantity to the right of the equality is because for the first half of the orbit, r˙ decreases as ψ increases. Bringing the term r2 under the square root gives: 1 dr =− dψ b

1/2 1/2 2 μ Ei r4 − r2 b2 − r4V (r) . μ

(1.71)

Dividing terms under the square root by η Ei b2 to bring this term out of the square root gives: dr 1 =− dψ b

4 1/2 1/2 r 2 V (r) (η Ei )1/2 b 2 1 − . − r2 μ b η Ei

(1.72)

1.2 Interactions Between Ions and Atoms

Since 1/2M1 2 = Ei , then = (2Ei /M1 )1/2 , and substituting for gives: 1/2 4 1/2 2 M1 dr r V (r) 2 =− η Ei 1 − − r dψ μ 2Ei b2 η Ei 1/2 4 1/2 M1 r V (r) 2 η =− 1 − − r μ b2 η Ei

4 1/2 r V (r) = − 2 1− . − r2 b η Ei

29

(1.73)

Substituting for x = 1/r gives:

1/2 1 dx V (x) 2 = 2 1− . −x dψ b η Ei

(1.74)

This is the equation of orbit (ψ = f (x)). The scattering angle φ is found by expressing dψ as a function of x and dx and integrating from the limits on ψ corresponding to x = 0 and 1/ρ . These limits are φ /2 and π /2, respectively, as shown in Fig. 1.10. Performing this integration for the first half of the orbit yields: π /2 φ /2

dψ =

1/ρ 1 0

1−

b2

−1/2 V (x) dx − x2 η Ei

(1.75)

and

φ = π −2

1/ρ 1 0

b2

1−

−1/2 V (x) dx . − x2 η Ei

(1.76)

The quantity ρ in the upper limit of x is the value of r when ψ = π /2 and hence is the distance of closest approach, Since dx/ dψ = 0 when ψ = π /2, ρ is given from Eq. (1.74) by:

η Ei =

V (ρ ) . b2 1− 2 ρ

(1.77)

Equations (1.76) and (1.77) provide the relation between φ and b. We have yet to determine the cross section for our scattering event. This may be done as follows. If particles M1 are bombarding target atoms M2 , then in Fig. 1.11, those ions which cross an area 2π b db enclosed by circles of radii b and b + db will be scattered into dφ about φ . Since the relation between db and dφ can be obtained from Eq. (1.76) by differentiation, the differential cross section is

30

1 The Radiation Damage Event

Fig. 1.11. Scattering of ions crossing an area 2π b db into an angular element dφ about φ

given by:

σ (Ei , T ) dT = 2π b db and σ (Ei , T ) = 2π b

db dφ . dφ dT

(1.78)

Knowing V (r) enables φ to be written in terms of b2 using Eq. (1.76) and then in terms of T using Eq. (1.13). Differentiating gives 2π b db as a function of T and dT . Then from Eq. (1.78) the differential cross section for collisions having recoils in dT about T follows. The total cross section for collisions with T anywhere in the range Tˇ to γ Ei is:

σ (Ei ) =

γ Ei Tˇ

σ (Ei , T ) dT .

(1.79)

The process for finding the energy transfer cross section can be summarized as follows: 1. 2. 3. 4.

Select a potential function V (r). Use Eq. (1.76) to obtain b as a function of φ , b = f (φ ). Use Eq. (1.13) to obtain φ as a function of T , φ = g(T ). Use the relations between b and φ and between φ and T in Eq. (1.78) to obtain the energy transfer cross section.

The preceding description of the energy transfer cross section emphasizes the importance of knowing the potential function describing the particular ion–atom or atom–atom interaction of interest. Without accurate knowledge of the potential function, further description of the collision process and the ensuing defect structure become impossible. Unfortunately, explicit evaluation of the integral in Eq. (1.76) is possible only for simple potential functions. But before looking further at the various potential functions and their application in determining the energy transfer cross section, we need first to consider the different possible classes of ions and their corresponding energies.

1.2 Interactions Between Ions and Atoms

31

Classification of Ions There are three important classes of ions in ion–atom collisions. The first is light energetic ions with Ei > 1 MeV. The second is highly energetic (Ei ∼ 102 MeV) heavy ions such as fission fragments (M ∼ 102 ). The third is lower energy heavy ions that may be produced by an accelerator or appear as a recoil that result from an earlier high-energy collision. The energy of these recoils is generally less than 1 MeV. For each of these interactions, we must decide on the most appropriate potential function. A convenient guide is ρ /a, the ratio of the distance of closest approach to the screening radius as a function of the recoil energy, T . A rough graph of ρ vs. T is provided in Fig 1.12 to aid in the selection of the most appropriate potential. The three curves represent ions of each of the three classes just discussed: (1) 20 MeV protons, (2) 70 MeV fission fragments, and (3) 50 keV Cu ions. Curve (1) collisions apply to the regime where ρ a and the simple Coulomb potential is adequate. Curve (2) collisions that are head-on will have ρ a also. But for glancing collisions, ρ ∼ a and the screened Coulomb potential is most appropriate. Curve (3) represents the region where a < ρ 5a and the inverse square potential or Brinkman potential would apply since both the Born–Mayer and screened Coulomb terms must be accounted for.

Fig. 1.12. Distance of closest approach r, as a function of T for (1) 20 MeV protons in Cu, (2) 70 MeV Xe+ ions in Cu, and (3) 50 keV Cu+ recoils in Cu (from [12])

32

1 The Radiation Damage Event

Hard-sphere Type Collisions The hard-sphere potential is appropriate for ion energies below about 50 keV and for near head-on elastic collisions. Here, ρ ∼ re and atoms will act like hard spheres. In a head-on collision, b = 0 and from Eq. (1.77) we have:

η Ei = V (ρ ) .

(1.80)

When b is not quite zero, the collision may be pictured as in Fig. 1.13 where we M2 M1 define R1 = ρ and R2 = ρ . If ρ is known, then from the figure: M1 + M2 M1 + M2 b = ρ cos

φ . 2

(1.81)

Now, recalling that:

σs (Ei , T ) dT = 2π b db db dφ , σs (Ei , T ) = 2π b dφ dT

(1.82)

2 db dφ = = 1/2ρ sin φ /2 from b = ρ cos φ /2, and from dφ dT γ Ei sin φ γ Ei ρ 2 (1 − cos φ ). Then σ (Ei , T ) = 2πρ cos φ /2 sin φ /2 , and T= 2 2 γ Ei sin φ

where

σs (Ei , T ) =

πρ 2 . γ Ei

(1.83)

Fig. 1.13. Schematic of colliding atoms obeying the hard-sphere approximation for collisions

1.2 Interactions Between Ions and Atoms

33

Recall that for neutron–nuclear interactions, σs (Ei , T ) = σs (Ei )/γ Ei . Using this relation, we can obtain an idea of the size of the energy transfer cross section σ (Ei , T )a−a = for neutron–nuclear interactions vs. atom–atom interactions: σ (Ei , T )n−nuclear πρ 2 π (10−8 )2 ∼ ∼ 108 , and so the energy transfer cross section for atom–atom σs (Ei ) 10−24 interactions is about eight orders of magnitude greater than that for neutron–nuclear interactions. The total scattering cross section is:

σs (Ei ) =

γ Ei Tˇ

σs (Ei , T ) dT =

γ Ei πρ 2 Tˇ

γ Ei

dT =

πρ 2 γ Ei − Tˇ = πρ 2 . γ Ei

(1.84)

Note that σs (Ei ) is independent of Ei (because ρ = f (Ei )), and that σs (Ei , T )α 1/Ei and is independent of T . We can find σs (Ei , T ) explicitly by applying the appropriate potential function to find a value of ρ (determined by V (r)). Recall from our discussions in Sect. 1.2.1 that for collisions in which the impact parameter is on the order of the equilibrium separation of the atoms, the Born–Mayer potential is most appropriate. This corresponds to energies below about 10 keV. (Note that this means that we are also backing off from a pure hard-sphere model.) Hence, we will use V (r) = A exp(−r/B), where A and B are defined in Eq. (1.47). Using Eq. (1.80) gives: V (ρ ) = A exp(−ρ /B) = η Ei or

ρ = B ln

A η Ei

(1.85)

,

(1.86)

and since b = ρ cos φ /2 = B ln(A/η Ei ) cos φ /2, the energy transfer cross section is:

σs (Ei , T ) =

π B2 A 2 . ln γ Ei η Ei

(1.87)

The total scattering cross section is then the integral of the energy transfer cross section between the limits Tˇ and γ Ei :

σs (Ei ) =

γ Ei Tˇ

A 2 1 π B2 ln dT . η Ei γ Ei

(1.88)

From this expression, we will be able to calculate the total cross section for displacement scattering events for all allowed T . Note that the total scattering cross section depends on Ei . Also, for typical values of A, B and Tˇ (25 eV), the value of σs (Ei ) for atom–atom interactions is about 108 times that for neutron–nuclear events.

34

1 The Radiation Damage Event

Rutherford Scattering Let us turn now to a second example in which we will use the pure Coulomb scattering potential to demonstrate Rutherford scattering. From our classification of ions according to ion energy and mass, type 1 collisions involve light (m ∼ 1 to 4) energetic (E > MeV) ions where ρ a. Collisions of this sort are adequately represented by the simple Coulomb potential, which from Eq. (1.48) is: V (r) =

Z1 Z2 ε 2 . r

We will assume that Z1 and Z2 represent the nuclear charges and that this collision occurs at high energies so that electrons are stripped from the nuclei and the only interaction is between the nuclei. In our description of the trajectories of the particles in the CM system, we found that at the point of closest approach, dx/ dψ = 0 and from Eq. (1.77):

η Ei =

V (ρ ) . b2 1− 2 ρ

Substituting in for V (r) gives: Z1 Z2 ε 2 b2 = η Ei 1 − 2 . ρ ρ Defining: Z1 Z2 ε 2 , b0 = η Ei

(1.89)

(1.90)

it follows that: b0 b2 = 1− 2 , ρ ρ

(1.91)

and

ρ=

1/2 4b2 b0 1+ 1+ 2 . 2 b0

(1.92)

Hence, the distance of closest approach is a function of the impact parameter b, as expected. For head-on collisions, b = 0 and the minimum value of ρ depends on Ei :

ρ (b = 0) = ρ0 = b0 =

Z1 Z2 ε 2 . η Ei

(1.93)

1.2 Interactions Between Ions and Atoms

35

Note that for this type of collision, ρ depends on Ei , in contrast to independence of Ei in the hard-sphere model. Going back to the orbital equation (1.75), we will now evaluate it as a definite integral: φ /2 π /2

dψ =

0

1

b2

1/ρ

−

b0 x − x2 b2

−1/2

dx .

(1.94)

Since ψ = π /2 when r = ρ (x = 1/ρ ) and ψ = φ /2 when r = ∞ (x = 0), letting b0 y = x + 2 , gives: 2b

φ /2 − π /2 = where

c2

=

b0 2b2 b0 1 ρ + 2b2

c2 − y2

−1/2

dy ,

(1.95)

b20 1 + . The orbits are then: b2 4b4

b y 02 φ /2 − π /2 = sin−1 2b c ρ1 + 2bb02

b0 b0 1 −1 1 . = sin − sin + 2b2 c ρ 2b2 1 b0 −1 1 + Since sin = sin−1 (1) = π /2, then: c ρ 2b2 −1

sin φ /2 =

b0 . 2b2 c

(1.96)

(1.97)

Substituting for c (from above) into Eq. (1.97) yields: sin2 φ /2 =

1 . 4b2 1+ 2 b0

(1.98)

Using trigonometric relations for sin2 φ /2, we have: b=

b0 cot φ /2 . 2

(1.99)

We now have a relationship between the impact parameter, b and the asymptotic scattering angle, φ . Note that b is a function of Ei through b0 (Eq. (1.93)).

36

1 The Radiation Damage Event

We now want an expression for the scattering cross section. Using Eq. (1.82) for σs (Ei , T ), we have:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ = 2π b db = π b0 cot

φ db , 2

(1.100)

and substituting for db from Eq. (1.99) gives:

σs (Ei , φ ) =

b0 4

2

1 , sin (φ /2)

(1.101)

4

which is the Rutherford inverse fourth power scattering law. The cross section for recoil is exactly the same as for elastic collisions, Eq. (1.13), and since:

σs (Ei , T ) = σs (Ei , φ )

dΩ , dT

we have:

σs (Ei , T ) =

π b20 Ei γ . 4 T2

(1.102)

Note that unlike neutron–nuclear collisions and hard-sphere scattering in general, the Rutherford scattering cross section is a strong function of T . This expression also shows that the scattering cross section σs (Ei , T ) → ∞ as T → 0. But this is just a reflection of the fact that as φ → 0, b → ∞ and is representative of longrange Coulomb interactions. In reality, there is a cut-off in b and hence in φ due to electron screening. As we will see later, this cut-off is Ed , the displacement energy. The average energy transferred is then: Tˆ

Tˇ ln(Tˆ /Tˇ ) ˇ T σs (Ei , T ) dT T¯ = T ˆ . = T Tˇ Tˇ σs (Ei , T ) dT 1− Tˆ For Tˆ = γ Ei and Tˇ = Ed and since γ Ei Ed , then: γ Ei T¯ ≈ Ed ln . Ed

(1.103)

(1.104)

which is quite small for all energies Ei , reflecting the strong 1/T 2 dependence in Eq. (1.102). The integral of Eq. (1.102) over T gives the total cross section for displacement events by an ion of energy Ei :

π σs (Ei ) = b20 Tˆ 4

Tˆ dT Ed

π b20 = T2 4

Tˆ −1 , Ed

(1.105)

1.2 Interactions Between Ions and Atoms

37

and since at high energies Tˆ /Ed 1 then we have for Tˆ = γ Ei :

σs (Ei ) ≈

π b20 γ Ei , 4 Ed

(1.106)

which is quite large. A critical question in applying the above results is under what conditions can Rutherford scattering be applied? The answer is that we must require that during an encounter, the major part of scattering occurs in the region where r a. But this is a qualitative measure. What is needed is a means for determining quantitatively, when Rutherford scattering applies. To address this question, we consider two cases. Case 1: Near “head-on” collisions high T . For near head-on collision, ρ0 a or Ei Ea , where Ea is the value of Ei that would give ρ0 = a assuming a screened Coulomb potential: Ea = 2ER (Z1 Z2 )7/6 (M1 + M2 ) /(M2 e) ,

(1.107)

which is obtained by re-writing the screened Coulomb potential (Eq. (1.49)) in an inverse square law form (Eq. (1.59)), with ε 2 = 2a0 ER and equating at r = a and M2 setting V (r) = η Ei = Ei for a head-on collision. M1 + M2 Case 2: Glancing collisions (low T). Here we only consider those collisions in which b ≤ a, or that result in an energy transfer Tˇ ∼ Ed for b = a. For a simple Coulomb collision with b = a, we have from Eqs. (1.98) and (1.13): T=

ε 2 γ Ea2 , 4Ei

or Ei =

ε 2 γ Ea2 , 4T

(1.108)

and giving this value of Ei the name Eb at T = Tˇ , we have Eb =

ε 2 γ Ea2 , 4Tˇ

where Tˇ = Ed ,

(1.109)

and this equation is valid for all Ei Eb . Essentially, Eb is the value of Ei that results in a transfer of energy T ≥ Ed at b = a. Or looking at it another way, values of Eb < Ei give T Tˇ and can be neglected since ρ ≥ a, and these encounters can be neglected. Table 1.4 provides examples of the values of Ea and Eb for different particle–target atom combinations and energies. From Table 1.4, since Ea < Eb , we can use the criterion that Ei must be Eb as an extreme test of the validity of the simple Coulomb scattering description. In summary, if Ei Ea , the simple Coulomb potential may be used for near head-on collisions. If Ei Eb , it can be used for all collisions of interest in radiation damage. Light charged particles such as protons and alphas with Ei > 1 MeV fall into this category, while fission fragments are in the regime Ea < Ei < Eb and recoils have Ei ≤ Ea . These will be discussed next. But first, we present an example of Rutherford scattering.

38

1 The Radiation Damage Event

Table 1.4. Values of Ea and Eb for various particle–target atom combinations and energies (from [13]) Incident particle C Al Cu Au Xe D+ D+ D+

Target atom

Ea (eV) 2 × 103

C Al Cu Au U C Cu U

1 × 104

7 × 104 7 × 105 5 × 105 1.5 × 102 1 × 103 4 × 103

Eb (eV) 8 × 105 2 × 107 1 × 109 1 × 1011 3 × 1010 2 × 103 2 × 104 1 × 105

Example 1.2. 2 MeV protons on aluminum For this case, Tˆ = γ Ei =

4(27) 2 MeV = 0.28 MeV (27 + 1)2

Tˇ = 25 eV

γ Ei T¯ = Ed ln Ed

= 233 eV

We can also calculate Ea ∼ 200 eV and Eb ∼ 4000 eV. (For comparison, 2 MeV He+ on Al, Ea ∼ 1 keV and Eb ∼ 25 keV. Also, for 2 MeV H+ on Au, Ea ∼ 1.6 keV and Eb ∼ 38 keV, and for 2 MeV He+ on Au, Ea ∼ 8 keV and Eb ∼ 69 keV.) Since Ei Eb , the simple Coulomb law is valid for this type of collision. Incidentally, σ (Ei ) ∼ 4 × 10−22 cm2 and since the mean free path between collisions is λ = 1/σ N and N ∼ 6 × 1022 a/cm3 , then λ ∼ 0.04 cm or about 400 μm, or about 10 times the length of a 2 MeV proton track in Al. This means that there is on average, only one Rutherford scattering collision for every 10 protons incident on Al.

Now, lets investigate the other classes of ion–atom collisions such as heavy, energetic ions, heavy, slow ions and high-energy electrons. Heavy, Energetic Ions For heavy, energetic ions such as fission fragments, Fig. 1.12 shows that an appropriate potential must account for both screened Coulomb and closed shell repulsion. Let us look first at the simple Coulomb potential as a rough approximation, knowing that its use is only justified for recoil energies approaching γ Ei which is where

1.2 Interactions Between Ions and Atoms

39

π b20 γ Ei 4M1 M2 M2 Z1 , and b0 α ,γ= ,η= , 2 4 Ed γ Ei M (M1 + M2 ) 1 + M2 which gives an increase in the cross section compared to the light ion by a factor of z21 M1 Ei heavy σheavy = 2 ≈ 106 σlight z1 M1 Ei

ρ a. Recall that σ (Ei ) =

light

light

for the fission fragments at the peaks of the fission yield of uranium, M1 96 amu, light heavy heavy E1 95 MeV and M1 137 amu, E1 55 MeV. Comparing to the example of the 2 MeV proton on Al, fission fragments have a cross section that is larger by a factor of 104 ! Therefore, the mean free path is 10−4 that of a proton in Al. Recall that σ (Ei , T ) varies as 1/T 2 . But this is only true near γ Ei (ρ a). At lower energies screening will reduce the sensitivity to energy. So we must use a better description of the interaction between energetic, heavy ions and target atoms. Brinkman’s expression, Eq. (1.50), includes both terms and if this is used in the impulse approximation (see [13]), the result is:

b b 2 M1 A2 , T= F α, − (1 − α ) F 1 + α , M2 Ei B B where A, B are given in Eq. (1.50) and − e−x dx b b ∞ = F α, B B b/a (x2 − b2/a2 )1/2 (1 − e−α x )2 b b ∞ (1 + nα ) , = ∑ (n + 1) K0 B n=0 B

(1.110)

(1.111)

where K0 (y) is a Bessel function of the third kind. The term α is the ratio of Born– Mayer and screened Coulomb terms at r = a, so in general, α < 1. T can be found from b and Eq. (1.110), and by inversion, b is obtained as a function of T . Differentiation gives σ = 2π b db. However, because of the complexity of Eq. (1.110), numerical solutions are required. Nevertheless, we may calculate dN, the number of recoils in dT at T produced by the fission fragment in slowing down to rest. This is found by: dσ dN = nσ dx = n dT

dE − dx

−1

dE dT ,

(1.112)

40

1 The Radiation Damage Event

Fig. 1.14. The energy spectrum of recoils N(T ) dT produced by fission fragments slowing down to rest in uranium. Two cases are shown: M1 = 96, E1 = 95 MeV and M1 = 137, E1 = 55 MeV (from [13])

where n is the density of atoms, and N (T ) dT = n

Ei σ dE −1 0

dT

dX

dE dT .

(1.113)

Brinkman carried out these calculations for light and heavy fragments from 235 U fission slowing down in uranium. The results are shown in Fig. 1.14. Note that N(T ) decreases more rapidly than T −1 and hence the majority of displaced atoms are produced by low-energy recoils. Therefore, high-energy recoils can be neglected altogether. Another way of looking at this is that the simple Coulomb potential is only valid in an energy range that does not contribute significantly to displacements. Heavy, Slow Ions These ions are classified by the curve labeled “3” in Fig. 1.12. This is a very important class of collisions as it covers most of the applications of kV ion implanters and low MeVaccelerators in the fields of materials science and radiation damage that includes such topics as ion implantation and heavy ion radiation effects simulation. The figure shows that collisions must be dealt with over the range a < ρ < 10a. The formalism used for fission fragments in the previous section applies to glancing collisions but for head-on collisions, another approach is needed. The appropriate

1.2 Interactions Between Ions and Atoms

41

potential for a/5 ≤ ρ ≤ 5a is the inverse square approximation. We use a potential of the form: a 2 2ER 0 (Z1 Z2 )5/6 , V (r) = e r which is obtained by fitting a screened Coulomb potential to the inverse square potential and equating at r = a, Eq. (1.59). Substituting this potential function into the orbital equation (1.76) gives: −1/2 φ a 2 Ea = 1− 1+ 2 . π b Ei

(1.114)

Using Eq. (1.13) to express φ in terms of T gives: −1/2 a 2 Ea 2 π T = γ Ei cos . 1+ 2 2 b Ei

(1.115)

Expressing b in terms of T and differentiating gives:

σs (Ei , T ) =

4Ea a2 α

γ Ei2 (1 − 4α 2)2 [x (1 − x)]1/2

,

(1.116)

T and πα = cos−1 x1/2 . γ Ei For small x (low-energy transfer), we have:

where x =

σs (Ei , T ) =

π 2 a2 Ea γ 1/2 1/2 3/2

8Ei

T

.

(1.117)

Note that the energy transfer cross section is dependent on T . The mean recoil energy is: γ Ei

1/2 ˇ T σs (Ei , T ) dT T¯ = T γ E = γ Ei Tˇ . i σ (E , T ) dT s i ˇ T

(1.118)

The total cross section for displacement is:

σs (Ei ) =

γ Ei Tˇ

π 2 a2 Ea γ 1/2 σs (Ei , T ) dT = 1/2 . 4 Ei Tˇ

(1.119)

Relativistic Electrons Radiation damage from electrons is not so important in reactor core materials, but more so in the laboratory as they are commonly used in electron microscopes for radiation damage studies. Due to the low mass of the electron, very high energies

42

1 The Radiation Damage Event

must be attained in order to cause displacements of a lattice atom. These energies are high enough such that relativistic quantum mechanics must be used to describe the collision. Even so, the energy transferred is large enough to displace only the struck atoms with no secondary displacements. In relativistic form, the momentum of an electron with rest mass m0 and kinetic energy Ei is: p2e =

Ei Ei + 2m0c2 . 2 c

(1.120)

Since the struck atom recoils non-relativistically, the recoil expression is that given in Eq. (1.9): 2 2 2 V2 = VCM + Vc2 − 2VCMVc cos φ = 2VCM (1 − cos φ ) = 4VCM sin2

φ , 2

and conservation of momentum gives: pe = (m0 + M) VCM ∼ = MVCM . Replacing the velocity terms with energies in the expression for V2 yields: T=

φ 2Ei Ei + 2m0c2 sin2 , 2 Mc 2

(1.121)

or 2Ei Tˆ = Ei + 2m0c2 . 2 Mc

(1.122)

An approximate expression for the Dirac equation for light ions [13] yields the differential scattering cross section:

σs (E1 , φ ) =

4π a20 Z22 ER2 1 − β 2 β4 m20 c4 2 2 × 1 − β sin (φ /2) + παβ sin (φ /2) (1 − sin (φ /2)) × cos (φ /2) csc3 (φ /2) ,

(1.123)

where β = v/c and α = Z2 /137. This expression approaches the Rutherford scattering law for small β . Using Eqs. (1.121) and (1.122), the differential scattering cross section is written in terms of T and Tˆ : 4π a20Z22 ER2 1 − β 2 T 1/2 T α Tˆ 2T σs (Ei , T ) = − . 1−β +π 2 4 4 β β T2 m0 c Tˆ Tˆ Tˆ (1.124)

1.2 Interactions Between Ions and Atoms

The total cross section is found by integrating Eq. (1.124) from Tˇ to Tˆ : 4π a20Z22 ER2 1 − β 2 Tˆ Tˆ 2 σs (Ei ) = β log − 1 − 2 4 β m0 c 4 Tˇ Tˇ 1/2 Tˆ Tˆ − 1 − log . +αβ 2 Tˇ Tˇ

43

(1.125)

For electrons with energies above the damage threshold and Tˆ /Tˇ slightly greater than unity:

σs (Ei ) ∼ =

4π a20Z22 ER2 m20 c4

1−β2 β4

2

Tˆ −1 . Tˇ

(1.126)

Figure 1.15 shows that at high enough energies, σ (Ei ) approaches an asymptotic value:

σs (Ei ) →

8π a20 Z22 ER2 Tˇ M2 c2

(1.127)

when Ei m0 c2 . It should be emphasized, however, that these cross sections are most accurate for light elements but seriously underestimate σs (Ei ) for heavy elements (Z > 50). Table 1.5 provides a summary of the energy transfer and the energy transfer cross sections for the various types of atom–atom interactions discussed in Sect. 1.2.

Fig. 1.15. Damage cross section for electrons bombarding copper where Ed = 25 eV (from [13])

44

1 The Radiation Damage Event

Table 1.5. Energy transfer and energy transfer cross sections for various types of atom–atom collisions Type of collision

Hard-sphere type (Born–Mayer potential) ρ ∼ re Rutherford scattering (simple Coulomb potential) ρ a Heavy ion (inverse square) a/5 ≤ ρ ≤ 5a Relativistic electrons

Energy transfer and energy transfer cross section

π B2 A 2 σs (Ei , T ) = ln γ Ei η Ei ¯ T = γ Ei /2

π b2 E γ σs (Ei , T ) = 0 i2 4 T γ E i T¯ ≈ Ed ln Ed σs (Ei , T ) =

π 2 a2 Ea γ 1/2 1/2 3/2

8Ei

Equation in text (1.87) (1.13) (1.102) (1.104) (1.117)

T

1/2 T¯ = γ Ei Tˇ 4π a20 Z22 ER2 1 − β 2 σ (Ei , T ) = β4 m20 c4 T 1/2 T T α Tˆ 2 +π × 1−β − 2 ˆ ˆ ˆ β T T T T

(1.118)

(1.124)

1.3 Ionization Collisions Up to this point, we have been treating collisions as discrete events. However, besides collision with or between nuclei, an ion or atom traveling through the lattice may lose energy by electronic excitation, by ionization or by Bremsstrahlung (loss of energy of an electron passing through the Coulomb field of a nucleus by emission of X-rays). These events may be viewed as more or less continuous events. What follows is a treatment of energy loss in solids. 1.3.1 Energy Loss Theory We are interested in finding the differential energy loss of an ion or atom traveling through a lattice. We begin by defining the energy loss per unit length as − dE/ dx (or NS(E) where N is the atom number density and S is the stopping power in units of energy × distance squared) so that the total energy loss can then be approximated by a sum of these components: dE dE dE dE = − + − + − , (1.128) − dx total dx n dx e dx r

1.3 Ionization Collisions

45

where the subscripts are defined as follows: n = elastic e = electronic r = radiation For most of the applications in which we will be interested, energy loss by radiation will be small and will be neglected. From our discussion in Sect. 1.2.1 it is evident that in order to accurately describe the slowing down of an ion or atom over the entire energy range from Tˆ to Tˇ , where Tˆ may be in MeVand Tˇ ∼ 10 eV, several potential functions would need to be “pieced” together (see Fig. 1.9). This would cause problems because of discontinuities at the cuts. Moreover, the cut-off points of these functions often differ depending on M and Z. However, we can separate or subdivide stopping power according to the type of interaction and hence, the energy regime. In the high-energy regime, ρ a and Se Sn and these interactions are treated as pure Coulomb collisions. In the lowenergy regime, ρ ≈ a and Sn > Se . This is the region of importance in the deposition of displacement energy. In either case, we can establish a formalism for calculating stopping power, dE/ dx = NS(E). If we know the energy transfer cross section σ (Ei , T ) for either Sn or Se , then we can calculate the average energy transfer:

T σ dT = energy lost or transferred, T¯ = σ dT 1 and the mean free path (mfp) between collisions is λ = σ . Then the ratio of these N two quantities is the energy loss per unit length:

Tˆ Tˆ dE T¯ ˇ T σ (Ei , T ) dT = = T ˆ σ (Ei , T ) dT ·N T dx λ Tˇ Tˇ σ (Ei , T ) dT

=N

Tˆ Tˇ

T σ (Ei , T ) dT ,

(1.129)

where N is the target number density. Another way to look at this is as follows: Consider a projectile incident on an amorphous target containing an average of N atoms/unit volume (Fig. 1.16). In traversing the slab of material between x and x + Δx, the projectile will come within a distance b1 of NΔx2π b1 db target particles and transfer an energy T (Ei , b) to each. The total energy transferred to all target particles in the slab is obtained by integrating over all possible impact parameters: ΔE = NΔx

∞ 0

T 2π b db.

46

1 The Radiation Damage Event Fig. 1.16. Schematic of an incident projectile of energy E passing within a distance b1 of an annular ring containing NΔx2π b1 db atoms

Assuming ΔE E and dividing by Δx and taking the limit as x → 0, we obtain: ∞ ΔE dE = N = T 2π b db. Δx lim x→0 dx 0 We know that σ (Ei , T ) dT = 2π b db, so: dE =N dx

Tˆ Tˇ

T σ (Ei , T ) dT ,

which is the same result as from Eq. (1.129). Let us first consider nuclear stopping, or energy loss from elastic collisions. Nuclear Stopping Power dE We define − or NSn (Ei ) as the energy lost to target nuclei when a projectile dx n of energy Ei traverses adifferential thickness dx of a target of unit density. A simple dE can be made if we assume that each target nucleus acts formulation of − dx n independently of every other target nucleus in slowing down a projectile. In essence, we are neglecting any possible interactions between nuclei. This is a fair approximation for amorphous targets and a good first approximation for crystalline targets also. Case 1: High-energy Elastic Collisions, ρ a. Rutherford scattering describes this type of interaction accurately. Recall that for simple Coulomb scattering, the energy transfer cross section (Eq. (1.102)) is:

σs (Ei , T ) =

π b20 γ Ei . 4 T2

1.3 Ionization Collisions

Therefore the stopping power becomes: γ Ei π b2 γ E dE = NS (E ) = N T 0 2i dT n i dx n 4 T Tˇ 2 N π b0 γ Ei = γ Ei ln , 4 Tˇ

47

(1.130)

ε 2 γ Ea2 where Tˆ = γ Ei and Tˇ is the value of T which yields b = a or Tˇb = . 4Ei Substituting for b0 from Eq. (1.93) gives: dE γ Ei N π Z12 Z22 ε 4 M1 = NS (E ) = ln . n i dx n Ei M2 Tˇb

(1.131)

Note that for like atoms, γ = 1 and M1 = M2 , so: NSn (Ei ) =

N π Z12 Z22 ε 4 Ei ln . Ei Tˇb

(1.132)

Substituting for Ea from Eq. (1.107) into the expression for Tˇb gives: 4E 2 (Z Z )2 (Z1 Z2 )2/6 Tˇb = R 1 2 . Ei

(1.133)

Using a = a0 /(z1 z2 )1/6 and substituting for (z1 z2 )1/6 gives: 4E 2 a2 Z 4 Tˇb = R2 0 , a Ei for z1 = z2 , and since ε 2 = 2a0 ER , then Eq. (1.132) becomes: 4N π Z 4 a20 ER2 Ei ln NSn (Ei ) = Ei Tˇb 2 2 4N π Z 4 a20 ER2 a Ei = ln Ei 4a20 ER2 Z 4

(1.134)

Case 2: Low-energy elastic collisions, ρ ∼ a. At intermediate and lower energies, pure Coulomb scattering will not correctly capture the interaction. Here we must use a screened Coulomb function to account for the effects of the electrons in the internuclear space. Lindhard, Nielsen and Scharff [14] proposed a universal, one-parameter, differential scattering cross section in reduced notation: −π a2 f t 1/2 σ= (1.135) 2 t 3/2

48

1 The Radiation Damage Event

where t is a dimensionless collision parameter defined by: t =∈2

T , Tˆ

(1.136)

and ∈ is dimensionless energy defined as: ∈=

aM2 Ei . Z1 Z2 ε 2 (M1 + M2 )

(1.137)

Lindhard et al. [14] treated f t 1/2 to be a simple scaling function where t was a measure of the depth of penetration into an atom during a collision and large t represents close approach. The function f t 1/2 is plotted as the thick solid line in Fig. 1.17. The analytical expression for the function developed by Winterbon et al. [15] is: −3/2 , (1.138) f t 1/2 = λ t 1/6 1 + (2λ t 2/3 )2/3 where λ = 1.309. A generalization of Eq. (1.138) for power law scattering is: 1 −m 1/2 = λm t 2 , f t

(1.139)

where λ1/3 = 1.309, λ1/2 = 0.327, and λ1 = 0.5. Equation (1.139) approximately describes scattering from a potential of the form V (r)α r−s = r−1/m , where s is the

Fig. 1.17. Reduced differential cross section calculated from the Thomas–Fermi potential. The thick solid line ranging over 10−3 M2 , B = 1/3. Increased electronic stopping at higher energies leads to smaller values of B. When M1 < M2 , large angle scattering

Fig. 1.23. Reduced range-energy plots for various values of the electronic stopping parameter, k

62

1 The Radiation Damage Event

increases the difference between R and Rp . However, for these collisions, electronic stopping is appreciable and partially offsets the increase in the difference. Therefore, B = 1/3 is a reasonable approximation for a wide range of conditions, giving: Rp ∼ =

R . 1 + (M2/3M1 )

(1.199)

Range straggling can be calculated using the theory of Lindhard et al. [16]. For the case where nuclear stopping dominates and M1 > M2 , i.e., small angle scattering: 1/2 M ) 2(M 1 2 ∼ 1.1Rp 2.5ΔRp = , (1.200) M1 + M2 or ΔRp ∼ = Rp /2.5 .

(1.201)

For a high-energy ion, the slowing down path is essentially a straight line in the original direction of motion, since the stopping is electronic with a small amount of straggle at the end due to nuclear collisions (Fig. 1.24a). At lower energies where Sn

Fig. 1.24. Total path length, projected range and perpendicular range for (a) high-energy ions and (b) low-energy ions incident on a target

1.3 Ionization Collisions

63

and Se are more comparable, the ion path follows a zigzag course with many large deflections with the distance between collisions decreasing as the energy decreases and the cross section increases (Fig 1.24b). The stopping positions are distributed according to a Gaussian as N(x) = Np e−1/2X , 2

(1.202)

x − Rp and ΔRp is the standard deviation (Fig. 1.25). If the peak conΔRp 1 centration is Np at Rp , then this will fall to 1/2 Np at distances x = Rp ± ΔRp . If we e view the target perpendicularly through its surface, then the number of implanted ions per unit area will be Ns , given by:

where X =

Ns =

+∞ −∞

N(x) dx ,

(1.203)

or since dx = ΔRp dX and the Gaussian curve is symmetrical, then: Ns = 2ΔRp Np

∞ 0

e−1/2X dX , 2

which can be written: √ 2 ∞ −1/2X 2 Ns = ΔRp Np 2π e dX . π 0

(1.204)

(1.205)

Fig. 1.25. Parameters of the Gaussian distribution applied to an ion implantation profile showing the projected range, R¯ p , the straggling or standard deviation, ΔRp , and the maximum concentration, Np of the implanted ion

64

1 The Radiation Damage Event

The integral inside the bracket is the error function and tends to unity as X → ∞, so that if Ns is the number of ions/cm2 implanted into the target, we have: Ns 0.4Ns ∼ Np = √ , = ΔRp 2π ΔRp so the density of implanted ions is: x − Rp 2 0.4Ns . N(x) = exp −1/2 ΔRp ΔRp

(1.206)

(1.207)

As an example, if we implant 5 × 1015 ions/cm2 of 40 keV B into Si, then Rp ∼ 160 nm, ΔRp ∼ 54 nm and Np ∼ 4 × 1020 atoms/cm2 . Note that from the properties of the Gaussian, the concentration will fall by one decade at x Rp ± 2ΔRp and by 2 decades at x Rp ± 3ΔRp, etc. Using the LSS treatment to describe electronic and nuclear stopping, Littmark and Ziegler have solved for the ranges of atoms with atomic number between 1 and 92 in all elements. Their work is published in Volume 6 of The Stopping and Ranges of Ions in Matter [20]. For each atom serving as the target, the mean ion depth, longitudinal straggling and transverse straggling is compiled in graphs for projectiles with 1 ≤ Z ≤ 92 and over a wide energy range. The following example is taken from this handbook.

Example 1.3. MeV He implantation into Si Zeigler [18] plots and tabulates the range parameters for a wide range of ions and target atoms. For 2 MeV He incident on a Si target, the range and straggling are 7.32 μm and 0.215 μm, respectively. If we assume a dose of 1015 He ions/cm2, then applying Eq. (1.204) gives a peak concentration of ∼1.86 × 1019 He atoms/cm3 at a depth of 7.32 μm, which is approximately 620 appm. Equation (1.205) gives the distribution of deposited He atoms as: x − 7.32 2 19 He/cm3 , N(x) = 1.86 × 10 exp −1/2 0.215 where x is in units of μm.

In addition to a tabulation of range data, Ziegler has developed a Monte Carlo based computer program for calculating the transport of ions in matter [18]. The program is available on the web at http://www.srim.org and the reader is encouraged to try some examples using the SRIM simulation software. This program is downloadable at no cost to the user (subject to the terms of use posted on the site) and may be executed on your personal computer. The following example uses data taken from the SRIM program.

1.3 Ionization Collisions

65

Example 1.4. Implantation of Al into Ni A similar example can be worked for lower energy implantation of a heavier element such as Al, into a nickel target. In this case, we use the output of the TRIM program. Selecting 200 keV Al in Ni results in a projected range of ∼135 nm with a longitudinal straggling of 44 nm. Substitution into Eq. (1.204) yields a peak concentration 9.1 × 1019 Al/cm3 for a dose of 1015 Al+ /cm2 . The TRIM software also yields a quantity that allows the user to determine concentration. The unit of concentration in the ion range plot is [atoms/cm3/atoms cm2 ] and the range of the implanted ion distribution on this plot has a maximum of ∼8 × 104 atoms/cm3 /atoms cm2 . Multiplying this value by the dose of 1015 Al+ /cm2 gives ∼8 × 1019 Al/cm3 which is close to the analytical solution.

Chapter Review The chapter began with a description of neutron–nuclear collisions, utilizing the absence of charge on the neutron to describe the interaction using a hard-sphere approximation. Expressions for the energy transfer in elastic and inelastic scattering collisions were developed and (n, 2n) and (n, γ ) reactions were analyzed as well to determine the energy transferred. Table 1.2 summarizes the energy transfer and energy transfer cross sections for these types of reactions. The description of projectile-target interaction was broadened to include ion–atom and atom–atom collisions which are relevant for two important cases: ion irradiation or implantation and the interaction between atoms in a lattice after the initial collision with a neutron in reactor materials. Interatomic potentials form the basis for describing the interaction between atoms and also for determining the energy transfer cross section. Table 1.3 summarizes the important potentials used to describe these interactions. Collision kinematics was then used to develop a description of the orbit of colliding atoms and hence, the transferred energy and the energy transfer cross section. Because there is not one single interatomic potential that describes the interaction over the entire distance (energy) range, the energy transfer and energy transfer cross sections are analyzed in various energy ranges and for various classes of interactions. Rutherford scattering is used to describe light energetic ions and slow heavy ions, energetic heavy ions, and relativistic electrons are all treated separately. Table 1.5 summarizes the energy transfer and energy transfer cross section for various atom–atom collisions. Energy loss theory is developed in order to determine the energy loss of energetic atoms/ions to the solid by elastic/nuclear collisions and by collisions with the electrons of the target. Collisions are analyzed in terms of their energy range for both nuclear stopping and electronic stopping. Table 1.7 summarizes the stopping

66

1 The Radiation Damage Event

powers for various types of interactions. Finally, the stopping powers are used to develop expressions for the range and projected range of ions in solids so that their penetration depth and concentration distribution can be determined.

Nomenclature a a0 aU A A b B C c D Ea Eb Ed ED Ef Eγ Ei f Ev,i m Ev,i Em Em EM EM ER ET I¯ m M N Np Ns pe Q re r˙ R Reff

Screening radius Bohr radius of the hydrogen atom Universal screening length Atomic mass Pre-exponential constant in Born–Mayer relation, Eq. (1.47) Impact parameter Constant in exponent in Born–Mayer relation, Eq. (1.47) Constant in screened Coulomb potential, Eq. (1.49) = 0.8853 Speed of light Nearest neighbor spacing between atoms Value of Ei that yields ρ0 = a Value of Ei that gives T ≥ Ed at b = a Displacement energy Maxwellian nuclear temperature = kT Final energy Gamma ray energy Incoming particle energy Vacancy and interstitial formation energy Vacancy and interstitial migration energy Kinetic energy of incoming particle in CM system Energy of neutron after (n, 2n) reaction Kinetic energy of target particle in CM system Energy of CM after (n, 2n) reaction Rydberg energy Total energy Excitation-ionization level Mass of incoming particle Mass of target Atom number density Peak implanted ion concentration Implanted ion density in ions/unit area Momentum of electron Excitation energy of nucleus Nearest neighbor spacing between atoms Radial velocity in polar coordinates Range of ion Recombination radius

Nomenclature

Rp ΔRp s Se Sn t t T Tˇ Tˆ T¯ T V (r) c Vc c Vc c Vc VCM V V Z

Projected range Standard deviation of projected range Power law exponent Electronic stopping power Nuclear stopping power Time Dimensionless collision parameter, Eq. (1.136) Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy transferred to target atom after (n, 2n) reaction Potential energy Velocity of incoming particle in CM system Velocity of target particle in CM system Velocity of incoming particle in CM system after collision Velocity of target atom in CM system after collision Velocity of neutron in CM system after (n, 2n) reaction Velocity of target atom in CM system after (n, 2n) reaction Velocity of CM in lab system Velocity of incoming particle in lab system Velocity of incoming particle in lab system after collision Velocity of target atom in lab system after collision Velocity of target atom in lab system after (n, 2n) reaction Atomic number

β χ (r) χU ε ∈ φ φ ψ˙ ψ λ λm λ μ ν (T ) θ ρ ρe ρ0 ρr

/c Screening function Universal screening function Unit charge Dimensionless, reduced energy parameter, Eq. (1.137) Asymptotic scattering angle at infinity separation Scattering angle in CM system Angular velocity in polar coordinates Scattering angle of struck atom in lab system Mean free path between collisions See Eq. (1.139) 1.309, Eq. (1.138) Reduced mass, Eq. (1.63) Displacement function Scattering angle in lab system Distance between atom centers in a collision Electron cloud density Distance of closest approach; value of r when ψ = π /2 Dimensionless, reduced distance parameter, Eq. (1.141)

67

68

1 The Radiation Damage Event

σ (Ei ) σ (Ei , T ) σ (Ei , φ ) σ (Ei , Eφ , Ω ) σ (Ei , Q j , φ ) σ (Ei , Q j , T ) Ω dΩ ξe

Total atomic collision cross section Differential energy transfer cross section Differential angular collision cross section Double differential collision cross section Differential angular cross section for inelastic collisions Differential energy transfer cross section for inelastic collisions Solid angle into which incoming particle is scattered Differential solid angular element 1/6 Z1

Problems 1.1 A 0.5 MeV neutron strikes a target atom with mass A, which is initially at rest. Calculate the velocity and energy of both particles in the laboratory reference frame after a head-on collision for A = 27 (Al) and A = 207.2 (Pb). 1.2 A detector of 100% efficiency (i.e., every particle entering the detector is registered) and area of 1 cm2 is placed a distance r from a target (taken to be of zero dimension, i.e., a point). The target is bombarded with neutrons. Assuming that only elastic scattering occurs, that scattering is azimuthally symmetric and that the scattering cross section is isotropic: a) What is the ratio of the number of particles detected by the detector at positions 1 and 2 shown in the figure? b) What is the ratio of the number of particles scattered through an angular increment of 10◦ about θ1 = 5◦ and θ2 = 85◦ ? c) Repeat parts (a) and (b) assuming that instead of being isotropic, the differential scattering cross section varies as σs (Ei , θ ) = cos θ .

dθ = Increment of scattering angle dΩ = Increment of solid angle about θ θ = Scattering angle in the center-of-mass system

Problems

69

1.3 A Ti plate is bombarded with 1014 neutrons per cm2 per second at perpendicular incidence. The entire plate is hit by the beam. a) Calculate the number of particles scattered per second at i) 85◦ ≤ θ = 86◦ and ii) 5◦ ≤ θ = 6◦ . The plate size is 1 cm2 by 0.6 mm. Scattering is isotropic with a total scattering cross section of 2.87 barns (1 barn = 10−24 cm2 ). b) The same target is bombarded with particles such that the differential angular scattering cross section is proportional to θ 2 . Calculate the ratio of the atomic flux in interval (i) above to that in interval (ii). In both cases, perform full integration of the differential cross section. c) Approximate the integrals in (b) by assuming the differential angular scattering cross section to be constant in each integration interval and equal to the value at the interval’s center. 1.4 Derive the kinematic factor K, defined as K = Ef /Ei , where Ei is the projectile energy before the collision and Ef is the projectile energy after the collision. 1.5 The following formula relates the scattering angles θ and φ in the lab and center-of-mass frames, respectively: tan θ = (M/m) sin φ / [1 + (M/m) cos φ ]

1.6 1.7 1.8

1.9

where m and M are the masses of the projectile and target, respectively. Discuss this expression for the following three cases: m = M, m M and m M. Derive Eq. (1.24) in the text. Derive Eq. (1.39) in the text. For two colliding particles write expressions for: a) ET , the total energy of a system of n particles b) ECM , the energy of the center of mass (determined by VCM and the total mass of the system) c) and E, the total energy in the CM system. Show that E = ET − ECM (Eq. (1.61)) Derive a relation between b and φ from Eq. (1.76) for the hard-sphere potential: VHS (r) = 0 =∞

r ≥ r0 r < r0

Make sure your answer is correct for b > r0 . 1.10 As a means of describing atom–atom interaction at intermediate separation, i.e., between Coulombic repulsion and closed shell repulsion, an inverse power potential is often employed of the form V (r) = constant/rn . For example, one can fit an inverse square (n = 2) function to the screened Coulomb potential at r = a obtaining the same slope, ordinate and curvature.

70

1 The Radiation Damage Event

This function is

V (r) = z1 z2 ε 2 a/ r2 exp[1] .

1.11

1.12

1.13

1.14

1.15

1.16

1.17

1.18

1.19

Formulate the cross sections σs (Ei , T ) and σs (Ei , φ ) for atom–atom interactions obeying the inverse square potential function. Compare your result in Problem 1.10 to that obtained using a Born–Mayer potential and a simple Coulomb potential. Comment on the similarities and differences. Calculate the average energy transfer from a 100 keV Ni atom colliding with another Ni atom, using: a) The hard-sphere potential b) The inverse square potential. Explain, in physical terms, why the scattering cross section resulting from Coulombic repulsion depends on the transferred energy, T , while that for neutron–nuclear interaction does not. Assuming a pure Coulomb potential, determine the distance of closest approach for a 100 keV boron atom on silicon for an impact parameter, b = 1 nm. What is the significance of your answer? 1 MeV Al+ ions are accelerated toward a pure Ni target. The ions are directed normal to the sample surface. a) Calculate the total path length and provide an estimate for the mean projected range of the ions. b) For a dose of 1016 ions/cm2 , estimate the maximum Al concentration and the FWHM of the Al distribution. Use Se = kE 1/2 , where k = 2 × 10−16 eV1/2 cm2 . A 10 MeV Si ion penetrates a Si crystal. a) Calculate its energy as a function of distance traveled and its penetration depth. Assume that electronic stopping dominates. b) Write an expression for the depth distribution of implanted Si ions and give the straggling. Calculate the energy threshold above which the Rutherford scattering cross section can be used for: (i) near head-on collisions, and (ii) all collisions of He++ and H+ in Si and Pd. 2 MeV He++ ions are backscattered (θ = 180◦ ) off of a 25 nm thick gold foil. Determine the highest and lowest energy values of the backscattered ions as measured in a detector placed at 180◦ with respect to the incoming beam. Use k = 0.14 × 10−15 eV1/2 cm2 . Determine the stopping power by interpolation or extrapolation based on the following values of 1/N( dE/ dx) (in eV/(1015 atoms/cm2)): Energy (MeV): 1.6 2.0 Au 122.3 115.5 Al 47.5 44.25 Assume the stopping power can be described by the following function: S = C + KE 1/2

where C and K are constants.

References

1.20 1.21

1.22

1.23

71

a) Derive an equation for the particle range as a function of energy. b) Does the range increase or decrease as: i) Energy increases ii) K increases iii) C increases. Which increases the high-energy electronic stopping power the most, increased charge, energy, or mass of the projectile ion? A 2 MeV proton travels through lead. a) Assuming elastic collisions, calculate the maximum energy that can be transferred from the proton to the lead. b) What energy would a Pb ion need to have the same maximum energy transfer in a Pb–Pb collision as the proton–Pb collision in part (a)? An Fe particle is fired at a block of natural uranium. To get the Fe as close to the uranium particle as possible, would you be better off using a higher charge state of Fe or a lighter isotope? Assume Coulomb potentials can be used. A thin film containing F19 is bombarded with 1.85 MeV protons. The following reaction takes place: F19 + p → O16 + α .

The reaction has a Q value of 8.13 MeV. After interaction, an alpha particle is seen to emerge at a right angle to the incident proton beam. What are the energies of the alpha particle and the oxygen atom? What is the maximum energy each of these particles could transfer to a stationary Fe atom? 1.24 A helium atom at 1 MeV is sent into iron. Assuming the electronic stopping cross section is a constant 88 eV/(1015 atoms/cm2 ), what is the energy of the helium atom after it travels 500 nm? If the He atom collides with an Fe atom after traveling 500 nm, what is the maximum energy transferred? Assume an atomic density of 8.5 × 1022 atoms/cm3 for Fe. Was an assumption of constant stopping power valid?

References 1. Ullmaier H, Schilling W (1980) Radiation damage in metallic reactor materials. In: Physics of Modern Materials, vol. I. IAEA, Vienna 2. Lamarsh JR (1971) Introduction to Nuclear Reactor Theory. Addison-Wesley, Reading, MA 3. Doran DG (1977) Nucl Sci Eng 49:130 4. Odette GR (1972) Trans Am Nucl Soc 15:464 5. Segev M (1971) Inelastic Matrices in Multigroup Calculation, ANL-7710. Argonne National Lab, Argonne, IL, p 374 6. Evans RD (1955) The Atomic Nucleus. McGraw-Hill, New York 7. Chadderton LT (1965) Radiation Damage in Crystals. Methuen, London

72 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20.

1 The Radiation Damage Event Born M, Mayer JE (1932) Z Physik 75:1 Firsov OB (1957) Zh eksper. teor. Fiz 32:1464 Firsov OB (1957) Zh eksper. teor. Fiz 33:696 Brinkman JA (ed) (1962) Radiation Damage in Solids. Academic, New York Abrahamson AA (1963) Phys Rev 130:693 Thompson MW (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge Lindhard J, Nielsen V, Scharff M (1968) Approximation method in classical scattering by screened Coulomb fields. Mat. Fys. Medd. Dan Vid. Selsk. 36(10) Winterbon KB, Sigmund P, Sanders JB (1970) Spatial distribution of energy deposited by atomic particles in elastic collisions. Mat. Fys. Medd. Dan Vid. Selsk. 37(14) Lindhard J, Scharff M, Schiott HE (1963) Range concepts and heavy ion ranges. Mat. Fys. Medd. Dan Vid. Selsk. 33(14):3 Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge Ziegler JF, Biersack JP, Littmark U (1996) The Stopping and Range of Ions in Solids. Pergamon, New York Lindhard J, Winther A (1964) Mat. Fys. Medd. Dan Vid. Selsk. 34:1 Littmark U, Ziegler JF (1980) Handbook of Range Distributions of Energetic Ions in all Elements. Pergamon, New York

2 The Displacement of Atoms

2.1 Elementary Displacement Theory The struck lattice atom of energy T , is referred to as a primary knock-on atom, or PKA. This atom moves through the lattice encountering other lattice atoms. Such encounters may result in sufficient energy transfer to displace this lattice atom from its site resulting in two displaced atoms. If this collision sequence continues, a series of tertiary knock-ons is produced resulting in a collision cascade. A cascade is a spatial cluster of lattice vacancies and atoms residing as interstitials in a localized region of the lattice. Such a phenomenon can have a profound effect on the physical and mechanical properties of the alloy, as will become evident later. Here we are concerned with being able to quantify the displacement cascade. That is, for a neutron of energy Ei , striking a lattice atom, how many lattice atom displacements will result? We have already discussed in detail the nature of neutron–nucleus and atom–atom collisions. Now, we will develop a model for determining the number of atoms displaced by a PKA of energy T . Recall that to quantify radiation damage, we require a solution to the damage rate equation: Rd = N

Eˆ Eˇ

φ (Ei ) σD (Ei ) dEi ,

(2.1)

where N is the lattice atom density, φ (Ei ) is the energy-dependent particle flux and σD (Ei ) is the energy-dependent displacement cross section. The displacement cross section is a probability for the displacement of lattice atoms by incident particles:

σD (Ei ) =

Tˆ Tˇ

σ (Ei , T ) ν (T ) dT ,

(2.2)

where σ (Ei , T ) is the probability that a particle of energy Ei will impart a recoil energy T to a struck lattice atom, and ν (T ) is the number of displaced atoms resulting from such a collision. Chapter 1 provided the energy transfer cross section appearing in Eq. (2.2) for various types of particles in various energy ranges. This chapter will be devoted to supplying the second term in the integrand, ν (T ), the number of atom displacements resulting from a primary recoil atom of energy T , and the limits of T between which displacements occur. Finally, we will develop the displacement cross section and an expression for the displacement rate.

74

2 The Displacement of Atoms

2.1.1 Displacement Probability As a first step, we define Pd (T ) as the probability that a struck atom is displaced upon receipt of energy T . Clearly, there is some minimum energy that must be transferred in order to produce a displacement. We will call this energy, Ed . The magnitude of Ed is dependent upon the crystallographic structure of the lattice, the direction of the incident PKA, the thermal energy of the lattice atom, etc. These considerations will be discussed in detail later. By definition of Ed , the probability of displacement for T < Ed is zero. If Ed is a fixed value under all conditions then the probability of displacement for T > Ed is one. Hence our simplest model for the displacement probability is a step function: Pd (T ) = 0 =1

for T < Ed for T > Ed .

(2.3)

and is shown in Fig. 2.1. However, Ed is not constant for all collisions due to the factors mentioned earlier. The effect of atomic vibrations of the lattice atoms would be expected to lower the value of Ed or introduce a natural “width” of the order kT to the displacement probability. Further, as will be discussed later, the effect of crystallinity will also contribute strongly to the blurring effect on Ed . In fact, the picture in Fig. 2.1 and Eq. (2.3) is only strictly true for an amorphous solid at 0 K. A more realistic representation is shown in Fig. 2.2 and is represented as: Pd (T ) = 0 = f (T ) =1

for T < Edmin for Edmin < T < Edmax for T > Edmax ,

(2.4)

where f (T ) is a smoothly varying function between 0 and 1. Given the displacement probability, the next task is to find the number of displacements as a function of the energy transferred. Kinchin and Pease [1] developed a simple theory to find the average number of displaced atoms initially created by a PKA of energy T in a given solid lattice. Their analysis is based on the following assumptions:

Fig. 2.1. The displacement probability Pd (T ) as a function of the kinetic energy transferred to a lattice atom, assuming a sharp displacement threshold

2.1 Elementary Displacement Theory

75

Fig. 2.2. The displacement probability as a function of the kinetic energy transferred to the lattice atom allowing for a blurring of the threshold due to atomic vibrations, impurity atoms, etc.

1. The cascade is created by a sequence of two-body elastic collisions between atoms. 2. The displacement probability is 1 for T > Ed as given by Eq. (2.4). 3. When an atom with initial energy T emerges from a collision with energy T and generates a new recoil with energy ε , it is assumed that no energy passes to the lattice and T = T + ε . 4. Energy loss by electron stopping is given by a cut-off energy Ec . If the PKA energy is greater than Ec no additional displacements occur until electron energy losses reduce the PKA energy to Ec . For all energies less than Ec electronic stopping is ignored, and only atomic collisions occur. 5. The energy transfer cross section is given by the hard-sphere model. 6. The arrangement of the atoms in the solid is random; effects due to crystal structure are neglected. Assumption 1 is fundamental to all theories of a cascade consisting of isolated point defects. Elimination of this restriction allows the cascade to be represented by a displacement spike discussed in Chapt. 3. Assumption 2 neglects crystallinity and atomic vibrations, which will add a natural width or “blurring” effect to the distribution. Later on, we will relax Assumptions 3, 4, 5 and 6. 2.1.2 The Kinchin and Pease Model for Atom Displacements Consider the two moving atoms created when a PKA first strikes a stationary atom. After the collision, the PKA has residual energy T − ε and the struck atom receives an energy ε − Ed , giving:

ν (T ) = ν (T − ε ) + ν (ε − Ed) ,

(2.5)

where Ed is the energy consumed in the reaction. By neglecting Ed relative to ε , i.e., ε Ed according to Assumption 3, then Eq. (2.5) becomes:

ν (T ) = ν (T − ε ) + ν (ε ) .

(2.6)

76

2 The Displacement of Atoms

Equation (2.6) is not sufficient to determine ν (T ) because the energy transfer ε is unknown. Since the PKA and lattice atoms are identical, ε may lie anywhere between 0 and T . However, if we know the probability of transferring energy in the range (ε , dε ) in a collision, we can multiply Eq. (2.6) by this probability and integrate over all allowable values of ε . This will yield the average number of displacements. Using the hard-sphere Assumption 5 the energy transfer cross section is:

σ (T, ε ) =

σ (T ) σ (T ) = γT T

for like atoms ,

(2.7)

and the probability that a PKA of energy T transfers energy in the range (ε , dε ) to the struck atom is: dε σ (T, ε ) dε = , (2.8) σ (T ) T and for γ = 1 (like atoms). Multiplying the right hand side of Eq. (2.6) by dε / dT and integrating from 0 to T yields:

1 T [ν (T − ε ) + ν (ε )] dε T 0

T T 1 = ν (T − ε ) dε + ν (ε ) dε . T 0 0

ν (T ) =

(2.9)

A change in variables from ε to ε = T − ε in the first integral and Eq. (2.9) gives:

1 T 1 T ν (ε ) dε + ν (ε ) dε , T 0 T 0 which is really a sum of two identical integrals. Therefore:

ν (T ) =

ν (T ) =

2 T

T 0

ν (ε ) dε .

(2.10)

(2.11)

Before solving Eq. (2.11), let us examine the behavior of ν (ε ) near the displacement threshold, Ed . Clearly when T < Ed there are no displacements and:

ν (T ) = 0 for 0 < T < Ed .

(2.12)

If T is greater than Ed but less than 2Ed , two results are possible. The first is that the struck atom is displaced from its lattice site and the PKA, now left with energy less than Ed , falls into its place. However, if the original PKA does not transfer Ed , the struck atom remains in place and no displacement occurs. In either case, only one displacement in total is possible from a PKA with energy between Ed and 2Ed , and:

ν (T ) = 1 for Ed < T < 2Ed .

(2.13)

Using Eqs. (2.12) and (2.13) we may split the integral in Eq. (2.11) into ranges from 0 to Ed , Ed to 2Ed , and 2Ed to T and evaluate:

E 2Ed T d 2 ν (T ) = 0 dε + 1 dε + ν (ε ) dε , T 0 Ed 2Ed

2.1 Elementary Displacement Theory

77

yielding:

ν (T ) =

2Ed 2 + T T

T 2Ed

ν (ε ) dε .

(2.14)

We can solve Eq. (2.14) by multiplying by T and differentiating with respect to T giving: T

dν =ν , dT

(2.15)

with the solution:

ν = CT .

(2.16)

Substituting Eq. (2.16) into Eq. (2.14) gives: C=

1 , Ed

(2.17)

and therefore:

ν (T ) =

T 2Ed

for 2Ed < T < Ec .

(2.18)

The upper limit is set by Ec (Assumption 4). When a PKA is born with T > Ec , the number of displacements is ν (T ) = Ec /2Ed for T > Ec . So the full Kinchin–Pease (K–P) result is: ⎧ ⎪ 0 for T < Ed ⎪ ⎪ ⎪ ⎪ 1 for Ed < T < 2Ed ⎪ ⎨ T ν (T ) = (2.19) for 2Ed < T < Ec . ⎪ 2Ed ⎪ ⎪ ⎪ ⎪ E ⎪ ⎩ c for T ≥ Ec 2Ed

Fig. 2.3. The number of displaced atoms in the cascade as a function of the PKA energy according to the model of Kinchin and Pease

78

2 The Displacement of Atoms

Note that T /2Ed is a true average since the number of displacements can range from 0 (no energy transfers above Ed ) to T /Ed − 1 (every collision transfers just enough) and for large T , ν approaches T /Ed . So the maximum value of ν (T ) is 2(T /2Ed) = T /Ed . The full displacement function described by Eq. (2.19) is shown in Fig. 2.3. 2.1.3 The Displacement Energy A lattice atom must receive a minimum amount of energy in the collision in order to be displaced from its lattice site. This is the displacement energy or displacement threshold, Ed . If the energy transferred, T , is less than Ed , the struck atom will vibrate about its equilibrium position but will not be displaced. These vibrations will be transmitted to neighboring atoms through the interaction of their potential fields and the energy will appear as heat. Hence, the potential fields of the atoms in the lattice form a barrier over which the stuck atom must pass in order to be displaced. This is the source of the displacement threshold energy. Since metals are crystallographic in structure, the potential barrier surrounding an equilibrium lattice site is not uniform in all directions. In fact, there are directions in which the surrounding atoms will remove large amounts of energy from the struck atom yielding a high potential barrier. Along directions of high symmetry there exist open directions along which the threshold displacement energy is low. Since the direction of the recoil is determined from the collision event which is itself a random process, the recoil direction is entirely random. The single value often quoted for displacement energy in radiation damage calculations then represents a spherical average of the potential barrier surrounding the equilibrium lattice site. The value of Ed may be roughly estimated using an argument by Seitz [2]. The energy of sublimation, Es , for most metals is about 5 – 6 eV. Since half as many bonds are broken by removing an atom from the surface of a crystal as opposed to the interior, the energy to remove an atom from the interior is then 10 – 12 eV. If an atom is moved from its lattice site to an interstitial position in the direction of least resistance and time is allowed for neighboring atoms to relax (an adiabatic movement), an energy of 2Ec is needed. Since in reality, the struck atom is not always projected in the direction of least resistance and time is not allowed for the relaxation of neighboring atoms, a greater amount of energy (perhaps 4–5 Ec ) is needed. Thus we would expect Ed to be 20 – 25 eV. Accurate determinations of the displacement energy can be made if the interaction potential between lattice atoms is known. This is accomplished by moving the atom in a given direction and summing the interaction energies between the moving atom and all other nearest neighbors along the trajectory of the struck atom. When the total potential energy reaches a maximum, the position corresponds to a saddle point and the difference between the energy of the atom at the saddle point, E ∗ , and its energy in the equilibrium position, Eeq , represents the displacement threshold for the particular direction. Since the interaction energy in these collisions is only tens of eV, the Born–Mayer potential would be the most appropriate potential to use in

2.1 Elementary Displacement Theory

79

describing the interaction. These calculations can be carried out over all directions and averaged to obtain a mean Ed for a particular solid. To appreciate the significance of the variation in interaction energies or potential barriers with crystal direction we will consider the case of copper. In the cubic lattice there are three crystallographic directions that may be considered easy directions for displacement; 100, 110 and 111. In particular, 110 is the closepacked direction in the fcc lattice and 111 is the close-packed direction in the bcc lattice. Figure 2.4 shows how an atom is displaced along each of these directions in the fcc lattice. In each case, the displaced atom K passes through the midpoint of a set of “barrier atoms” B, in the direction of the L atom, with the atom configuration dependent on the direction. For a K atom displaced in the 110 direction, the atoms are located at the corners of a rectangle to which the path of K is perpendicular. When the K atom passes through the barrier, it loses kinetic energy in glancing collisions, which initially becomes potential energy of the barrier atoms. The energy need not be shared equally between the four B atoms. This is illustrated by drawing a set of contours of constant Ed in the place of the B atoms (Fig. 2.5). Then if K only receives a quantity of energy Ed 110 in the collision event, it will be displaced if its initial direction is contained within a small cone of solid angle centered about the 110 direction. For small energies, the cone intersects the B atom plane in a circle but as the energy transferred increases, the intersection deviates significantly from a right circular cone (Fig. 2.5). The contours are in fact, generated by the intersection of a complex but symmetrical three-dimensional surface with a sphere which is described about the atom K as center. This contour pattern can be constructed by accounting for the interaction between the K atom

Fig. 2.4. Struck atom, K, and barrier atoms B for various directions of the struck atom in the fcc lattice

80

2 The Displacement of Atoms Fig. 2.5. Equipotential contours in the barrier plane for a struck atom, K, traveling close to the 110 direction and heading toward the barrier plane defined by the barrier atoms, B (after [3])

and each of the B atoms at every point in time while simultaneously accounting for interactions between each of these five atoms and other atoms in the surrounding region of the crystal. This is a very difficult problem, the solution of which depends heavily on the interaction potential. In principle, at least, we can obtain all the information we need about the directional dependence of the thresholds. Figure 2.6 shows the displacement threshold as a function of direction in fcc copper and gold. Note that displacement threshold energies along 100 and 110 are low, but the value along 111 is high due to the large distance between barrier atoms in this direction and the two sets of barriers between the atoms on the body diagonal of the unit cell. This dependence will be further illustrated in an example using the fcc lattice and a parabolic repulsion function. Figure 2.7 shows a lattice atom on the face of a unit cell in an fcc crystal receiving energy from a collision. Its flight trajectory is in the 100 direction, which is equidistant from four atoms located on the faces of the unit cell. In an fcc lattice, each atom is surrounded by 12 nearest neighbors. Displacement will be dependent on several important factors. They are the number of barrier atoms, B, the impact parameter, z (the distance of closest approach to the B atoms), and the distance from the K atom in its lattice site to the barrier, y. These quantities are given in Table 2.1 for the fcc lattice. The energy required to displace an atom will increase with B and y and decrease with z. Since z is smallest for the 111 direction, this will be the most difficult to penetrate. Also z100 < z110 and y100 > y110 , so both factors will make displacement along 110 easier then along 100. Lets take the specific example of displacement in the 100 direction of the fcc example and calculate a value for Ed . The energy of a single atom in a normal lattice site is: Eeq = −12U ,

(2.20)

2.1 Elementary Displacement Theory

81

Fig. 2.6. Displacement energy as a function of direction in (a) fcc Cu and Au crystal (after [3]), and (b) in copper (after [4])

where U is the energy per atom of the crystal. Since only half as many bonds are broken in the sublimation process, this energy is just: Es ∼ = 6U ,

(2.21)

and since Es ∼ 4 – 5 eV, U is about 1 eV. To describe the interaction of the lattice atoms as they are pushed together in the solid, we will use a simple parabolic repulsion as opposed to the Born–Mayer

82

2 The Displacement of Atoms

Fig. 2.7. Displacement of a lattice atom along the 100 direction in the fcc lattice and the variation of energy of the atom with position along its path (after [5])

potential: 1 V (r) = −U + k(req − r)2 2 V (r) = 0 r > req ,

r < req (2.22)

where k is the force constant characterizing the repulsive position of the potential. The force constant can be expressed as [5]: ka2 =

3v , β

(2.23)

where k a v = a3 /4 β

= force constant = lattice constant = specific volume of an atom = compressibility.

In our example, the equilibrium spacing of the struck atom and the four atoms form√ ing the square barrier is req = a/ 2. When the atom is at the center of the square, it interacts with the four atoms at the corners a distance a/2 away. Hence, the energy Table 2.1. Parameters used for the determination of Ed in the fcc lattice Direction

# B atoms

Impact parameter, z

Distance to barrier, y

100

4

a 2 √

110

4

111

3

a 2√ 2 a 4 a 3

6 a 4 a √ 6

2.1 Elementary Displacement Theory

83

Table 2.2. Recommended values of the effective displacement energy for use in displacement calculations (from [6]) Metal

Lattice (c/a)

Al Ti V Cr Mn Fe Co Ni Cu Zr Nb Mo Ta W Pb Stainless steel

fcc hcp (1.59) bcc bcc bcc bcc fcc fcc fcc hcp bcc bcc bcc bcc fcc fcc

Ed,min (eV)

Ed (eV)

16 19 – 28 – 20 22 23 19 21 36 33 34 40 14

25 30 40 40 40 40 40 40 30 40 60 60 90 90 25 40

at the saddle point is:

1 1 2 1 2 = 4 −D + (ka ) √ − . E = 4V 2 2 2 2 ∗

a

(2.24)

The displacement energy in the 100 direction is then: 1 1 2 . Ed 100 = ε ∗ − εeq = 8D + 2 ka2 √ − 2 2

(2.25)

Typical values for ka2 and U for metals are 60 eV and 1 eV, respectively, yielding Ed 100 ∼ = 13.1 eV. This value is in reasonable agreement with that given in Fig. 2.6. Table 2.2 gives values of Ed for various metals [6]. Note that for the transition metals, the accepted value of Ed is 40 eV. 2.1.4 The Electron Energy Loss Limit Now that we have established a lower limit on the energy transfer necessary to cause a displacement, Ed , lets turn our attention to the high-energy regime of collisions. Recall that at low energies (T < 103 eV), Sn Se , and we may assume that nearly all of the energy loss of the PKA goes toward elastic collisions (Fig. 1.18). However, as the PKA energy increases, the fraction of the total energy loss that is due to electron excitation and ionization increases until above the crossover energy, Ex , Se > Sn .

84

2 The Displacement of Atoms

Fig. 2.8. Energy loss from electronic and nuclear stopping as a function of energy (after [7])

Our expression for ν (T ) in Eq. (2.19) must therefore be modified to account for this variation in the amount of kinetic energy available for displacement collisions. Figure 2.8 shows ( dE/ dx)n for carbon recoils in graphite using Eq. (1.162) and Lindhard’s Thomas–Fermi result, the latter showing that Eq. (1.162), which predicts a constant value of 250 eV/nm is a good approximation for energies up to at least Ea . Note that at high energies (T Ex ) electronic energy losses predominate by several orders of magnitude. However at low energies (T Ex ) the situation is reversed. Fortunately, because of departures from the hard-sphere model, the primary re1 coil creates secondaries with average energies far below Tˆ . These will almost 2 always be in the range where electronic excitation can be neglected. To obtain ν (T ) to a fair approximation we calculate the energy Ec , dissipated in elastic collisions by the PKA: Ec =

Tˇ 0

( dE/ dx)n dE . ( dE/ dx)n + ( dE/ dx)e

(2.26)

We can then use Eq. (1.182) for ( dE/ dx)e and Eq. (1.130) for ( dE/ dx)n with Tˇ = Ea . The modified damage function is the original Eq. (2.19) with T replaced by Ec :

ν (T ) =

Ec . 2Ed

(2.27)

2.2 Modifications to the K–P Displacement Model

85

Fig. 2.9. Number of displaced atoms per primary recoil compared to the simple K–P result of T /2Ed (after [7])

As an estimate of Ec we can use the maximum energy a moving atom (of energy E) can transfer to an electron as: 4me E, M

(2.28)

and equating this with the ionization energy of the struck electron belonging to the target atom we have: Ec =

M I. 4me

(2.29)

Kinchin and Pease [1] equated Ec and Ex , implying that all energy above Ex is lost in electron excitation, and displacements account for all the energy loss below Ec . Figure 2.9 shows ν (T ) for graphite using Lindhard’s ( dE/ dx)n . Note that for recoils with energy below Ec , the simple theory gives a fair description, but for T > Ec , the losses in electron excitation are important.

2.2 Modifications to the K–P Displacement Model 2.2.1 Consideration of Ed in the Energy Balance Snyder and Neufeld [8] make the assumption that an energy Ed is consumed in each collision such that the relation in Assumption 3 of the K–P displacement model will

86

2 The Displacement of Atoms

read: T = T + ε + Ed ,

(2.30)

and both atoms move off after collision, no matter how small their energy. When compared with the Kinchin–Pease model, it may be expected that ν (T ) would decrease since an energy loss term is added. However, because atoms are allowed to leave the collision with energy less than Ed , an increase in ν (T ) will occur. Since these two changes to ν (T ) nearly cancel, the result is very similar to the K–P model: T ν (T ) = 0.56 1 + (2.31) for T > 4Ed . Ed 2.2.2 Realistic Energy Transfer Cross Sections The weakest point of the K–P displacement model is the assumption of hard-sphere collisions (Assumption 5). In fact, more realistic energy transfer cross sections can be used while still maintaining the proportionality of Eq. (2.19). Sanders [9] solved Eq. (2.5) using an inverse power potential (r−s ) to obtain: 1

T ν (T ) = s 2 s+1 − 1 , 2Ed

(2.32)

which for the inverse square potential becomes:

ν (T ) = 0.52

T , 2Ed

(2.33)

reducing the Kinchin–Pease result by a factor of 2. However, the use of this potential has its shortcomings because it is applied to all collisions in the cascade while its region of validity is limited to those values of T such that ρ < 5a. Physically, the effect of realistic scattering is to make a larger number collisions generate T in the subthreshold regions below Ed where they are removed from multiplication chain. For many years, investigators have been intrigued that Eq. (2.19) appears to overestimate ν (T ) in metals by a factor of 2 to 10 [10] and yet attempts to measure the energy dependence of ν (T ) over a large energy range (50 – 200 keV recoil atoms in gold) gave a quadratic rather than linear relationship. In 1969 Sigmund [11] took a different approach to this problem by considering the recoil density F(T, ε ) dε defined as the average number of atoms recoiling with an energy in (ε , ε + dε ) as a consequence of a primary ion slowing down from T to zero energy. The recoil density can be expressed in a form that uses the power law approximation of the Thomas–Fermi differential cross section [12]:

σ (T, E) ∝ T −m ε −1−m ,

(2.34)

2.2 Modifications to the K–P Displacement Model

87

where 0 ≤ m ≤ 1, giving: F(T, ε ) =

T m , ψ (1) − ψ (1 − m) (ε + U)1−m ε 1+m

(2.35)

for T ε U, where

ψ (x) = d[ln Γ (x)]/ dx ,

(2.36)

U is the binding energy lost by an atom when leaving a lattice site, and Γ (x) is the gamma function or the generalized factorial function. Since a recoiling atom is displaced when ε > Ed we obtain:

ν (T ) =

T Ed

dε F(T, ε ) =

(1 + U/Ed)m − 1 T ψ (1) − ψ (1 − m) U

(2.37)

for T Ed U. The value of m is chosen in such a way [13] that σ (T, ε ) describes collisions at low energies, i.e., 2Ed ≤ T ≤ 100Ed. This constrains m ≤ 4. For m = 0, Eq. (2.37) reads:

ν (T ) =

6 T ln(1 + U/Ed) . π2 U

(2.38)

This is an upper limit for displacement processes since loss of defects by replacement collisions has been neglected. A characteristic feature of displacements in metals is the large recombination volume of an isolated point defect, of the order of 100 atomic volumes or more. Hence, Ed is the energy lost to the environment by an atom trying to escape the recombination volume. This has the consequence that in cascades, many defects are lost by replacement collisions [14]. The binding energy U is only a few eV and thus negligible as compared to Ed , reducing Eq. (2.38) to: T 6 T ν (T ) = 2 = 1.22 , (2.39) π Ed 2Ed which is about 22% greater than the result of Eq. (2.19) which accounted for replacement collisions. 2.2.3 Energy Loss by Electronic Excitation Even for E > Ec , collisions of the PKA with electrons compete for energy loss against collisions with lattice atoms. These two processes can be treated independently, and each can be represented by separate energy transfer cross sections. The formulation originally presented by Lindhard et al. [15] is summarized here as presented by Olander in [5] as a more realistic treatment of energy loss by electronic excitation (Assumption 4).

88

2 The Displacement of Atoms

As a PKA traverses a distance dx of a solid, three things may happen: (1) it collides with an electron, (2) it collides with an atom, or (3) nothing. Let pe dεe be the probability that a collision between the PKA and an electron in the interval dx transfers energy in the range (εe , dεe ) to the electron: pe dεe = N σe (T, εe ) dεe dx ,

(2.40)

where σe (T, εe ) is the energy transfer cross section from the PKA to the electron. Similarly, for a PKA and lattice atom: pa dεa = N σa (T, εa ) dεa dx ,

(2.41)

and the probability that nothing happens in dx is: po = 1 −

εe,max 0

pe dεe −

εa,max 0

pa dεa

(2.42)

= 1 − N dx[σe (T ) − σa (T )] , and εe,max , εa,max are the maximum energies transferable to an electron and atom by a PKA of energy T . We re-write the conservation equation for ν (T ) by weighting with the appropriate probability for the process by which it is created and integrating over the permissible ranges of energy transfers:

ν (T ) =

εa,max 0

+

[ν (T − εa ) + ν (εa )]pa dεa

εe,max 0

(2.43)

ν (T − εe )pe dεe + p0 ν (T ) .

Substituting for pe , pa and p0 yields: [σa (T ) + σe (T )]ν (T ) =

εa,max 0

+

[ν (T − εa ) + ν (εa )]σa (T, εa ) dεa

εe,max 0

ν (T − εe )σe (T, εe ) dεe .

(2.44)

Since the maximum energy transferred to an electron is very small compared to T , ν (T − εe ) can be expanded in a Taylor series and truncated after the second term:

ν (T − εe ) = ν (T ) −

dν εe , dT

(2.45)

and the last term in Eq. (2.44) can be written as: εe,max 0

ν (T − εe )σe (T, εe ) dεe = ν (T ) −

dν dT

εe,max 0

σe (T, εe ) dεe

εe,max 0

εe σe (T, εe ) dεe .

(2.46)

2.2 Modifications to the K–P Displacement Model

89

The first integral on the right in Eq. (2.46) is the total cross section for collisions of the PKA with the electron, and cancels the corresponding term on the left in Eq. (2.44). The second integral on the right of Eq. (2.46) is the electronic stopping power of the solid divided by the atom density. Substituting Eq. (2.46) using Eq. (2.45), we have:

Tmax ( dT / dx)e dν σ (T, ε ) = ν (T ) + [ν (T − ε ) + ν (ε )] (2.47) dε , N σ (T ) dT σ (T ) 0 where the subscript “a” on T and σ has been dropped with the understanding that these quantities refer to atomic collisions. (2.47) can be solved us Equation dE is given by Eq. (1.182), i.e., ing the hard-sphere assumption, but where dx e dE = kE 1/2 , giving: dx e

ν (T ) =

2Ed 2 + T T

T 2Ed

ν (ε ) dε −

kT 1/2 dν . σ N dT

After simplification, the final result is:

T 4k ν (T ) = 1 − , 2Ed σ N(2Ed )1/2

for T Ed ,

(2.48)

(2.49)

where k is a constant depending on the atom number density, N, and the atomic number. The term σ is the energy-independent hard-sphere collision cross section. Note that when electronic stopping is properly accounted for in the basic integral equation, the entire concept of a definite energy, Ec , separating regimes of electronic energy loss from atomic collisions can be dismissed. However, Eq. (2.49) is still plagued by the use of the hard-sphere assumption. Lindhard realized that in order to ensure that reliable predictions are obtained, a realistic energy transfer cross section must be used. Lindhard also realized that the parameter ν (T ) need not be interpreted solely as the number of displacements produced per PKA, but could be taken to be that part of the original PKA energy, which is transferred to the atoms of the lattice (rather than the electrons) in slowing down. In reality, collisions of the PKA with atoms compete with collisions with electrons. But the processes can be treated as independent events. Nevertheless, the expression for ν (T ) needs to be reformulated. According to Lindhard’s energy partitioning theory: T ν (T ) = ξ (T ) , (2.50) 2Ed where

ξ (T ) =

1 1/6 3/4 1 + 0.13(3.4εT + 0.4εT + εT )

,

(2.51)

90

2 The Displacement of Atoms

εT is a reduced PKA energy: εT =

T , 2Z 2 ε 2 /a

(2.52)

and a is the screening radius a=

0.8853a0 . Z 1/3

The damage energy efficiency function ξ (T ) is given as a function of PKA energy, T , and as a function of Z (various elements) in Fig. 2.10. In 1975, Norgett, Robinson and Torrens [17] proposed essentially this model to calculate the number of displacements, Nd according to: Nd =

κ ED κ (T − η ) = , 2Ed 2Ed

(2.53)

where T is the total energy of the PKA, η is the energy lost in the cascade by electron excitation, and ED is the energy available to generate atomic displacements by elastic collisions, and is known as the damage energy. The displacement efficiency, κ is 0.8 and is independent of M2 , T or temperature. The quantity ED is defined by: ED =

T , [1 + kNg(εN )]

(2.54)

Fig. 2.10. The effect of electronic energy losses on the energy available for atomic displacements (from [16])

2.2 Modifications to the K–P Displacement Model

91

and inelastic energy loss is calculated according to the method of Lindhard using a numerical approximation to the universal function, g(εN ): 1/6

3/4

g(εN ) = 3.4008εN + 0.40244εN + εN 1/2 1/6 Z1 kN = 0.1337Z1 A1 A2 T a εN = (A1 + A2) Z1 Z2 ε 2 2 1/3

9π 2/3 2/3 −1/2 a0 Z1 + Z2 a= 128

(2.55)

where a0 is the Bohr radius and ε is the unit electronic charge. If Ed ∼ 40 eV, then Nd = 10ED , where ED is in keV. 2.2.4 Effects of Crystallinity The analysis thus far has assumed that the cascade occurs in a solid composed of a random array of atoms. However, when the order of a crystal structure is imposed (Assumption 6), two important effects occur that can alter the number of displacements produced by a PKA; focusing and channeling. Focusing is the transfer of energy and/or atoms by near head-on collisions along a row of atoms. Channeling is the long-range displacement of atoms along open directions (channels) in a crystal structure in which an atom travels by making glancing collisions with the walls of the channel which are just rows of atoms. Both processes can result in long-range transport of interstitials away from the initial PKA or the cascade. Both processes also reduce the number of displacements per PKA, ν (T ), as calculated from the simple Kinchin–Pease model. Focusing The effects of focusing were first seen in the directional dependence of the threshold energy, Ed . In an fcc lattice, for example, displacements occur in the 100 and 110 directions with the lowest energy transfer of any crystalline direction. Since the direction of the primary knock-on is random, focusing must be possible for a sizable range of polar angles off the close packed direction. If exact head-on collision were required to produce a linear collision chain, the phenomenon would be of little practical significance since this probability is extremely low. Focusing along an atomic row can be analyzed using the hard-sphere approximation. The distance between atoms along a particular crystallographic is denoted by D. Figure 2.11 shows two atoms of such a row in which a collision sequence is initiated by the atom which was initially centered at A. This atom receives energy T and moves off at an angle θ0 to the atomic row. The dashed circle shows the atom position at the instant it strikes the next atom in the row. The radius of the colliding

92

2 The Displacement of Atoms

Fig. 2.11. The simple focusing effect assuming hard-sphere collisions

sphere, R, is obtained from the Born–Mayer potential. The impact transfers some of T to the second atom, which then moves off in the direction of the line joining P and B at an angle θ1 to the row. From Fig. 2.11 we can also show that: AP sin θ0 = PB sin θ1 .

(2.56)

If θ0 and θ1 are small, Eq. (2.56) can be approximated by: APθ0 ≈ PBθ1 ,

(2.57)

and if θ0 and θ1 are very small, then AP ≈ AB − PB = D − 2R , and since PB = 2R (D − 2R)θ0 = 2Rθ1 , and

θ0 (D − 2R) = θ1 (2R) .

(2.58) (2.59)

If we further define a focusing parameter: f ≡ θ1 /θ0 ,

(2.60)

then by Eq. (2.59): f=

D −1 . 2R

(2.61)

This permits us to write the following inequalities: for f > 1 ,

D > 4R

and |θ0 | < |θ1 |

for f < 1 ,

D < 4R

and |θ0 | > |θ1 | .

(2.62)

2.2 Modifications to the K–P Displacement Model

93

Considering further collisions, by the time the momentum pulse reaches atom n, the relation between angles is given by:

θn = f θn−1 = f 2 θn−2 = f 3 θn−3 (2.63)

: :

= f θ0 = n

D −1 2R

n

θ0 ,

or finally

θn = ( f ) θ0 = n

D −1 2R

n

θ0 .

(2.64)

This last relation shows that if D > 4R, the focusing parameter f is greater than unity so that the angles θn will increase in successive collisions. Conversely, if D < 4R, f is less than unity and the angles θn converge to zero. A set of conditions also exist under which the scattering angle θn will neither diverge nor converge after successive collisions. These are the conditions for critical focusing (θn = θn+1 = . . .) which can be determined as follows. The recoil angle of atom B can be related to the initial direction of atom A by applying the law of sines to triangle APB: D sin(π − θ0 − θ1 ) , = sin θ0 2R

(2.65)

which simplifies to: D sin(θ0 + θ1 ) . = sin θ0 2R

(2.66)

The condition for critical focusing is θ1 = θ0 . Applying this equality in Eq. (2.66) gives: sin 2θ0 D , = 2 cos θ0 = sin θ0 2R

(2.67)

and cos θ0 = cos θc =

D , 4R

or focusing will occur when cos θ0 ≤ cos θc =

D . 4R

(2.68) D and 4R (2.69)

94

2 The Displacement of Atoms

Equation (2.60) also shows that focusing of momentum is favored along rows of atoms in the hkl directions for which the separation distance Dhkl is a minimum, or the close-packed directions. If we treat the atoms as having an energy-dependent radius, we can determine the maximum possible energy for focusing at any given collision angle. The key is to allow the potential between atoms to vary with separation. The critical focusing energy, Efhkl , is defined as that energy below which f < 1, D < 4R and focusing is possible. In the hard-sphere model the relation between kinetic energy E, and 1 potential energy V (r) for a head on collision is given by Eq. (1.80) as V (2R) = E. 2 If V (r) is given in the Born–Mayer potential, Eq. (1.47), V (r) = A exp(−Br), then: E = 2A exp(−2R/B) .

(2.70)

For a head-on collision, θc = 0, so cos θc = Efc = 2A exp

−D 2B

D = 1, and we have: 4R

.

(2.71)

This means that any angle greater than zero will result in defocusing for E ≥> Ec , or that focusing at an energy Efc can only occur for θ = 0◦ . Clearly then, the critical focusing angle depends on the energy of the projectile. The relation between angle and energy is developed by writing the expression for Efc in terms of D: 2A D = 2B ln . (2.72) Efc Now, for any atom of energy T reaching a separation of 4R gives: 2A 4R = 2B ln . T

(2.73)

Combining these equations gives: ln(2A/Efc ) D = cos θc = , 4R ln(2A/T )

T < Efc .

(2.74)

Note that the condition of critical focusing can be expressed in two ways: −D : This condition gives the energy Efc for which focusing 1. Efc = 2A exp 2B occurs for a head-on collision (θc = 0). ln(2A/Efc ) : This condition gives the maximum angular deviation from 2. cos θc = ln(2A/T ) a head-on collision θc , at which a PKA of energy T can initiate a focused sequence.

2.2 Modifications to the K–P Displacement Model

95

From the first expression, it should be apparent that focusing is a function of crystallographic direction since D is a function of crystal structure. That is: −Dhkl Efhkl = 2A exp . (2.75) 2B For example, in the fcc lattice, we have: D100 = a √ 2 a D110 = 2 √ D111 = 3a 110

100

111

therefore, since D110 < D100 < D111 , we have Ef > Ef > Ef . 110 in copper and 600 eV for gold. In any Typical values for Ef are 80 eV for Ef case, Ef is much less than initial PKA energies. From the preceding discussion, it should be apparent that focusing is only applicable if a scattered atom is within an angle θc of an atomic row. Then a focused sequence can result. It is therefore important to determine the probability that the initial direction of a struck atom is within a cone of apex θc about an atomic row. For a random starting direction, the probability of generating a focused collision sequence at energy T is: Pf (T ) =

θc2 . 4

(2.76)

Expanding cos θc in Eq. (2.69) gives: 1 D , for small θc . Substituting from Eq. (2.75) gives: 1 − θc2 ≈ 2 4R 1 D Pf (T ) = 1− 2 4R or

1 ln(2A/Efc ) 1− 2 ln(2A/T )

ln(2T /Efc ) 1 . = 2 ln(Efc /2A) + ln(T /Efc )

(2.77)

Pf (T ) =

(2.78)

Since Efc /2A 1 and T /Efc ∼ 1, then: 1 ln(T /Efc ) 2 ln(Efc /A) = 0 T > Efc

Pf (T ) =

T < Efc

(2.79)

96

2 The Displacement of Atoms

For n equivalent directions in the crystal: Pf (T ) = n

ln(T /Ec ) . ln(Ec /A)

(2.80)

For example, in copper Efc ∼ 80 eV, and for A ∼ 20,000 eV, Pf (60 eV) ∼ 0.026n. For n = 12, then Pf ∼ 0.3 or 30%. Focusing refers to the transfer of energy by elastic collisions along a line, but without involving the transfer of mass. We will next discuss replacement collisions in which both energy and mass are transferred. Replacement Collisions In addition to energy transfer, mass can be transferred by replacement of the struck atom with the striking atom if the center of the first atom moves beyond the midpoint of the two atoms as they reside in the lattice. In our analysis of focusing we assumed hard-sphere collisions. However, if we assume that there is a softness to the atom, three things occur: 1. The hard-sphere model overestimates the angle of scattering for a particular impact parameter and hence the amount of focusing must be overestimated. 2. Atoms is the row feel the influence of the oncoming disturbance long before it gets there so the atom is already moving. Since D is decreased, focusing is enhanced. 3. Replacement becomes possible. Referring to Fig. 2.12, as the collision proceeds, the distance x between atoms An and An+l decreases continuously. The velocity of the center of mass (CM) is: M1 M2 VCM = 1 + 2 , M1 + M2 M1 + M2 where 1 and 2 are in the lab system. The relative speed, defined by g = 1 − 2 gives: M2 1 = VCM + g M1 + M2 M1 g, 2 = VCM + M1 + M2 and the total kinetic energy of the two particles is: KE = 1/2M1 21 + 1/2M222 , and in terms of g and VCM is: 2 + 1/2μ g2 , KE = 1/2(M1 + M2 )VCM M1 M2 where μ is the reduced mass = . The total kinetic energy is divided into M1 + M2 two parts: one due to the motion of the system and another due to the relative motion

2.2 Modifications to the K–P Displacement Model

97

Fig. 2.12. Head-on collisions in a focused chain when the interaction potential acts continuously during the collision. (a) Atom positions during the collision initiated by the atom on the left. (b) Separation of atoms An and An+1 during the collision (after [5])

of the two particles. Conservation of total energy is given as Er +V (x) = Er0 , where V (x) is the potential energy at a head-on separation distance of x, Er0 is the relative kinetic energy at infinite (initial) separation, and Er is the relative kinetic energy at any point. Rewriting the kinetic energy in terms of g gives: 1 1 2 μ g + V (x) = μ g20 2 2 and g0 = 10 , where g0 is the initial speed. This equation should be recognizable from our earlier analysis in Chap. 1, Sect. 1.2.2. Recall that at x = xmin , V (xmin ) = 1/2 μ g20, and for M1 = M2 , then g0 = 10 and V = E/2. We also assume that the interaction energy at the initial separation is V (D) 1 2 . The time rate of change of the separation distance is equal to the relative μ g 0 2 speed: dx = −g . dt

(2.81)

98

2 The Displacement of Atoms

Taking the collision time as twice the time needed to reach the distance of closest approach: tc = −2

xm dx

g

D

= −2

V (xm ) V (D)

dV , g dV / dx

(2.82)

where xm is the distance of closest approach. Since V (x) = A exp(−x/B), then dV A V = − exp(−x/B) = − , dx B B

(2.83)

and:

1/2 1 2 4 g= μ g0 − V (x) 2 M 1/2

4 E −V = 2 M E V 1/2 − =2 , 2M M

(2.84)

where μ = M/2 for like atoms and 1/2μ g20 = 1/4M210 = E/2. Substitution of Eqs. (2.83) and (2.84) into Eq. (2.82) yields:

2M 1/2 E/2 dV tc = B E V (D) V (1 − 2V/E)1/2

2M 1/2 2V (D) 1/2 tanh−1 1 − . = 2B E E

(2.85) (2.86)

Note that the definition of a hard-sphere radius has been used for the upper limit, i.e., xm is taken to be 2R(E). For V (D)/E 1, tc = B

2M E

1/2 ln

2E . V (D)

Since the speed of the center of mass is

(2.87) 10 = 2

E 2M

1/2 , the distance moved by

the CM during the collision time, tc , is: x = tc

E 2M

1/2 .

(2.88)

If x > D/2, atom An will end up to the right of the initial halfway point and replacement will occur and An will occupy the lattice site occupied by atom An+1 . Relating

2.2 Modifications to the K–P Displacement Model

99

Fig. 2.13. Energy scale for focused energy transfer and focused replacement sequence

the distance x to energy by substituting for tc from Eq. (2.87) into Eq. (2.88) gives: 2Er x = ln . (2.89) B V (D) For x = D/2: D 2Er , = exp 2B A exp(−D/B) and the replacement energy becomes: −D A Er = exp . 2 2B

(2.90)

According to the above arguments, and comparing to Eq. (2.71), focused replacement is possible when the energy transported in the collision chain satisfies: −D 1 1 = Efc . (2.91) E > Er = A exp 2 2B 4 Therefore, we get focused replacement, or Efc /4 < T < Efc : focused replacement T < Efc /4 : focused momentum/energy packet . Hence mass transfer can occur when E is between Er = Efc /4 and Efc , which from our previous example is about the same or slightly less than the displacement energy, Ed . Figure 2.13 shows where focusing and replacement collisions fall on the energy spectrum of the PKA. Assisted Focusing In our analysis of focusing, we have not accounted for the effects of surrounding atoms or nearest neighbors. Due to their repulsion of the moving atom, they tend to act as a lens and aid in the focusing process. The net result of this assisted focusing is to increase the critical energy for focusing, Efc , rendering focusing more probable. Second, the ring of atoms surrounding a focusing event also tend to dissipate energy by glancing collisions. This effect is augmented by the vibrational motion of the atom rings, which can be increased with temperature. The length of

100

2 The Displacement of Atoms

the replacement chain and the number of collisions in the chain decrease as the temperature increases. The increased motion of the surrounding atoms increases the energy loss from the collision sequence. Other effects that destroy the sequence are alloying elements and defects such as interstitials, vacancies and dislocations. Figure 2.14 shows the number of collisions in a focused chain of initial energy E in room-temperature copper along with the focusing probability. Table 2.3 from Chadderton [18] gives the focusing and replacement energies in various directions in fcc and bcc lattices as modified by surrounding atoms (assisted focusing). Note that in all cases, the focusing energies are larger when the surrounding atoms aid in the focusing process.

Fig. 2.14. Length and probability of the collision chain in a 110 collision sequence in copper at room temperature (after [5]) hkl ) in the fcc and bcc lattices (after [18]) Table 2.3a Equations for focusing energies (Efc

hkl Face-centered cubic

Body-centered cubic

↑ A(D110 )2 D110 exp − 4B 2D2 D110 110 2A exp − 2B 1/2 ↑ 6 D110 19 1/2 A(D110 )2 A 111 exp − 19 2B 12 D2

D111 2A exp − √ B 3 √ ↑↑ √ D111 5 4 2(D111 )2 A exp − √ 15B2 2 3B 111 D 2A exp − 2B

100

2.2 Modifications to the K–P Displacement Model

101

Table 2.3b Equations for replacement energies (Erhkl ) in the fcc and bcc lattices (after [18]) hkl

Face-centered cubic D110 100 5A exp − √ D 2 D110 A exp − 110 2 2B D110 111 4A exp − √ B 3 ↑ In the (110) plane only ↑↑ Assisted focusing

Body-centered cubic D100 A exp − 2 2B D110 3A exp − 2B D111 2A exp − 2B

Channeling Channeling is the long distance displacement of energetic knock-on atoms down an open direction in the crystal lattice. Figure 2.15a shows a schematic of an atom spiraling down an open channel in a crystal lattice and Fig. 2.15b shows axial and planar channels along specific crystallographic directions in the fcc lattice. The walls of the passageway consist of atomic rows. If the rows surrounding the channel are close-packed, discrete repulsive forces between atoms are “smeared out” and the atom appears to be traveling in a long cylindrical tube with radius Rch . The value of Rch can be determined by equating π R2ch with the cross sectional area of the channel. If the amplitude of the lateral oscillations of the moving atom is small compared to Rch , the potential well provided by the channel wall is roughly parabolic in the direction transverse to the channel axis. The interaction of the moving atom with a channel wall (Fig. 2.16) can be described by a harmonic channel potential: Vch (r) = kr ,

(2.92)

where r is the lateral distance from the axis, and k is the force constant which depends on the potential function describing atom–atom repulsion and channel dimension Rch . Using the Born–Mayer potential to describe atom–atom interactions in this energy regime, k becomes: −Rch A 2π Rch k= exp , (2.93) DB B B where D is the atom spacing in the rows forming the channels. Moving atoms enter the channel with a velocity component along the channel axis (Fig. 2.16) given by: 1/2 2E cos θ0 , (2.94) Vz0 = M where (2E/M)1/2 = V0 . The axial velocity is gradually reduced by inelastic energy loss to the electron cloud. The moving atom undergoes simple harmonic motion in

102

2 The Displacement of Atoms

Fig. 2.15. (a) Schematic of an atom moving in a channel in a crystal lattice (after [19]). (b) Axial and planar channels in the fcc lattice (after [20])

2.2 Modifications to the K–P Displacement Model

103

Fig. 2.16. Trajectory of a channeled atom (after [5])

the r direction with period τ given by: 1/2 M τ = 2π 2k and the initial wavelength of the oscillation is equal to Vz0 τ for θ0 = 0 or: 1/2 E λ = 2π . k

(2.95)

(2.96)

The amplitude of lateral oscillation is determined by the injection angle, θ0 and the kinetic energy of the injected atom, E. The r component of the atom velocity as it enters the channel is: 1/2 1/2 2E 2E ∼ Vr0 = sin θ0 = θ0 . (2.97) M M So the radial component of the kinetic energy is E θ02 , which is equal to the potential 2 . Equating kinetic and potential energies energy at the transverse amplitude, krmax and solving for rmax gives: 1/2 E rmax = θ0 , k and the trajectory of the channeled atom is: 1/2 1/2 k E r = θ0 sin Z . k E

(2.98)

(2.99)

104

2 The Displacement of Atoms

The critical angle beyond which channeling cannot occur, θch , is obtained by equating the transverse amplitude, rmax , and the channel radius, Rch : 1/2 k θch = Rch . E

(2.100)

Note that θch decreases as E increases, as expected. When the mean free path between collisions is of the order of a few atom spacings, large-angle collisions become probable and channeling dissipates. The channeling probability is difficult to determine since we must knock an atom into the channel, but there are no atoms near the channel axis. The event probably starts with an impact on an atom forming the channel wall. If the entrance angle is small enough, it may begin to channel. There is no upper limit on energy for channeling. Instead, θch just becomes smaller as E increases. The minimum channeling energy occurs when the wavelength is ∼ nD or a few atom spacings (n ∼ 2). Essentially, there develops a resonance between impulses from channel walls and transverse oscillations. The trajectory terminates in a violent collision. Recall that our treatment is only valid if λ D. Solving for E in Eq. (2.96) and letting λ = 2D yields Ech ∼ 0.1 kD2. For copper, Ech is about 300 eV. Ech is larger for large mass because k increases with mass. Channeling is a high-energy phenomenon and is most significant for light atoms, while focusing is a low-energy phenomenon that is most significant for heavy atoms. Effect of Focusing and Channeling on Displacements The probability of a crystal effect is a function of recoil energy. P(T ) is used for either Pf or Pch , but since Ef ∼ 100 eV, Pf is quite small. The equation governing cascade effects can be modified to account for crystal effects by modifying Eq. (2.14):

2Ed 2 T + ν (T ) = P(T ) + [1 − P(T)] ν (ε ) dε . (2.101) T T 2Ed The first term on the right in Eq. (2.101) represents the lone displaced atom, which results if the PKA is channeled or focused on the first collision. The second term gives the number of displacements created by a PKA that makes an ordinary displacement on the first collision. Assuming P = P(T ), Eq. (2.101) is differentiated with respect T to yield: T

dν = (1 − 2P)ν + P . dt

(2.102)

Integration gives

ν (T ) =

CT (1−2P) − P 1 − 2P

(2.103)

2.3 The Displacement Cross Section

105

Fig. 2.17. Energy scale showing focused energy transfer, focused replacement sequence and channeling

and the constant C can be found by substitution into Eq. (2.82): C=

1−P , (2Ed )(1−2P)

resulting in the final solution: T (1−2P) 1−P P . ν (T ) = − 1 − 2P 2Ed 1 − 2P For small P, ν (T ) can be approximated by: T (1−2P) ν (T ) = . 2Ed

(2.104)

(2.105)

It should be noted that the most important crystal effect is channeling which is most important at high energies. For example, for P = 7%, a 10 keV PKA in iron produces 100 displacements or about half the amount with P = 0. Figure 2.17 shows where channeling occurs on the PKA energy scale. Note that channeling is a high-energy phenomenon and that there is a gap between the replacement energy, below which replacements or focused energy transfer occur, and the channeling energy, above which channeling occurs. Given the K–P model for displacement and the various modifications to the basic model, we now turn to the determination of the number of displaced atoms.

2.3 The Displacement Cross Section The results of previous sections may now be used to define the displacement cross section as:

σD (Ei ) =

Tˆ Tˇ

ν (T )σ (Ei, Q j , T ) dT ,

(2.106)

106

2 The Displacement of Atoms

where ν (T ) is the number of displacements caused by a PKA of energy T , σ (Ei, Q j , T ) is the general form of the energy transfer cross section, and Tˇ and Tˆ are the minimum and maximum transfer energies. This quantity was first presented in Eq. (2.2) and gives the average number of displacements produced by an incoming neutron of energy Ei . We can apply this expression to the various regimes of scattering in order to determine their individual contributions to the total number of displacements. We will first determine σD (Ei ) for each type of interaction using the basic K–P result and then go back and add in the modifications. 2.3.1 Elastic Scattering Consider σs (Ei , T ) for elastic scattering. From Eq. (1.19),

σs (Ei , T ) =

4π σs (Ei , φ ) . γ Ei

In the case of isotropic scattering:

σs (Ei , φ ) =

σs (Ei ) ; 4π

therefore:

σs (Ei ) σDs (Ei ) = γ Ei

γ Ei Ed

σs (Ei , T ) =

σs (Ei ) , γ Ei

ν (T ) dT .

(2.107)

Should we wish to consider anisotropic elastic scattering in systems such as fast reactors, the angular dependence of the elastic scattering cross section can be written in a series of Legendre polynomials:

σs (Ei , φ ) =

σs (Ei ) ∞ ∑ a(Ei )P(cos φ ) , 4π =0

(2.108)

where σs (Ei ) is the total elastic scattering cross section for incident neutrons of energy Ei , P is the th Legendre polynomial, and values of a are the energy-dependent coefficients of the cross section expansion. At neutron energies encountered in thermal or fast reactors, it is sufficient to retain only the first two terms, = 0 and = 1. Since P0 = 1 and P1 = cos φ :

σs (Ei , φ ) =

σs (Ei ) [1 + a1(Ei ) cos φ ] . 4π

(2.109)

Also, given that cos φ = 1 − 2T /γ Ei , and substituting Eq. (2.109) into Eq. (2.106) gives:

2T σs (Ei ) γ Ei σDs (Ei ) = ν (T ) 1 + a1(Ei ) 1 − dT . (2.110) γ Ei E d γ Ei

2.3 The Displacement Cross Section

107

2.3.2 Inelastic Scattering Since inelastic scattering is isotropic in the center-of-mass system:

σs j (Ei , Q j , φ ) =

σs j (Ei , Q j ) . 4π

(2.111)

Equation (1.30) gives the energy transfer cross section for inelastic scattering in the resonance region as:

σs j (Ei , Q j ) Qi 1 + A −1/2 σs j (Ei , Q j , T ) = , 1+ γ Ei Ei A so that

σDs j (Ei ) = ∑ j

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj 1+ ν (T ) dT , γ Ei Ei A Tˇ j

(2.112)

where the minimum and maximum values of T (Ei , Q j , φ ) are given by Eq. (1.27) and setting cos φ = −1 and 1, respectively, gives: 1/2 Q Q 1 + A γ E 1 + A j j i 1+ + 1+ Tˆj = 2 2A Ei Ei A 1/2 Q Q 1 + A γ E 1 + A j j i 1+ − 1+ Tˇ j = . 2 2A Ei Ei A 2.3.3 (n, 2n) and (n, γ ) Displacements The displacement cross section for (n,2n) reactions can be written as:

σD(n,2n) (Ei ) =

Ei −E m 0

σ(n,2n) (Ei T )

T dT , 2Ed

(2.113)

where σ(n,2n) (Ei , T ) is given by Eq. (1.40). The displacement cross section due to (n, γ ) reactions can be written as:

σDγ (Ei ) = σγ

Tˆ T 0

2Ed

dT .

(2.114)

However, since we have assumed that the lattice atom recoils with an average energy T=

Eγ2 Tˆ = , 2 4(A + 1)c2

and that Eγ for a given isotope is either known or can be measured, Eq. (2.114) can be simplified to:

σDγ = σγ

Eγ2 T = . 2Ed 8Ed (A + 1)c2

(2.115)

108

2 The Displacement of Atoms

The total displacement cross section due to these forms of neutron interaction then becomes:

σD (Ei ) =σDs (Ei ) + σDs j (Ei ) + σD(n,2n) (Ei ) + σDγ

2T σs (Ei ) γ Ei T = 1 + a1(Ei ) 1 − dT γ Ei Ed 2Ed γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T dT +∑ 1+ γ Ei Ei A Tˇ j 2Ed j +

Ei −E m 0

+ σγ

σ(n,2n) (Ei , T )

Eγ2 , 8Ed (A + 1)c2

T dT 2Ed (2.116)

where the terms are for elastic scattering, inelastic scattering in the resonance region, (n,2n) reactions and (n,γ ) reactions, respectively. 2.3.4 Modifications to the K–P Model and Total Displacement Cross Section The displacement cross section can be modified to account for the relaxation of the various assumptions made to the basic K–P model as in Sect. 2.2. These modifications are as follows summarized in Table 2.4. Applying these correction terms to the basic K–P result by consolidating Assumptions 1 and 3 into a single constant C and using Eq. (2.104) for the effect of crystallinity, transforms Eq. (2.116) to read: σs (Ei ) γ Ei 1 − P T (1−2P) P σD = − C ξ (T ) γ Ei E d 1 − 2P 2Ed 1 − 2P

2T × 1 + a1(Ei ) 1 − dT γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 +∑ 1+ γ Ei Ei A j Tˆj T (1−2P) P 1−P dT × − C ξ (T ) 1 − 2P 2Ed 1 − 2P Tˇ j Ei −E m 1−P T (1−2P) P + dT σ(n,2n) (Ei , T ) − C ξ (T ) 1 − 2P 2Ed 1 − 2P 0 ⎤ ⎡ 1−2P 2 E 1−P P ⎦ γ + σγ ⎣ . (2.117) C ξ (T ) − 1 − 2P 8Ed (A + 1)c2 1 − 2P

2.4 Displacement Rates

109

Table 2.4. Modifications to the displacement cross section Assumption 3: Loss of Ed 4: Electronic energy loss cut-off 5: Realistic energy transfer cross section 6: Crystallinity

Correction to ν (T ) T 0.56 1 + 2E d T ξ (T ) 2Ed T , 0.52 < C ≤ 1.22 C 2Ed 1−P P T (1−2P) − 1 − 2P 2Ed 1 − 2P T (1−2P) ∼ 2Ed

Equation in text Eq. (2.31) Eq. (2.50) Eqs. (2.33), (2.39)

Eq. (2.104) Eq. (2.105)

Using the more simplified expression for the effect of crystallinity Eq. (2.104) reduces Eq. (2.117) to: (1−2P)

σs (Ei ) γ Ei T 2T σD = C ξ (T ) 1 + a1(Ei ) 1 − dT γ Ei E d 2Ed γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T (1−2P) dT +∑ 1+ C ξ (T ) γ Ei Ei A 2Ed Tˇ j j Ei −E m T (1−2P) + σ(n,2n) (Ei , T ) C ξ (T ) dT 2Ed 0 1−2P Eγ2 , (2.118) + σγ C ξ (T ) 8Ed (A + 1)c2 or,

σD = σDs + σDi + σD(n,2n) + σDγ .

(2.119)

The displacement cross section for stainless steel was calculated by Doran [21] using the energy partition theory of Lindhard and is shown in Fig. 2.18.

2.4 Displacement Rates Recall that the displacement rate was given in Eq. (2.1) as: R=

Tˆ Tˇ

N φ (Ei )σD (Ei ) dEi .

This is the displacement rate density or total number of displacements per unit volume per unit time [#/cm3 s]. To get a rough estimate of the order of magnitude of

110

2 The Displacement of Atoms

Fig. 2.18. The displacement cross section for stainless steel based on a Lindhard model and ENDF/B scattering cross sections (after [21])

this number, let us simplify the displacement cross sections as follows. Neglecting (n,2n) and (n,γ ) contributions to displacements, all modifications to the simple K–P displacement model (i.e., using ν (T ) = T /2Ed ), and neglecting Ed relative to Ei , the displacement cross section due to elastic and inelastically scattered neutrons only becomes:

2T σs (Ei ) γ Ei T σD (Ei ) = 1 + a1(Ei ) 1 − dT γ Ei Ed 2Ed γ Ei

(2.120) σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T +∑ dT . 1+ γ Ei Ei A Tˇ j 2Ed j Assuming that elastic scattering is isotropic (a1 = 0), neglecting inelastic scattering and integrating between the limits Ed and γ Ei gives:

σD (Ei ) =

σs (Ei ) γ Ei

γ Ei T Ed

2Ed

dT ,

and if γ Ei > Ec , then:

2E Ec γ Ei d σs (Ei ) T Ec σD (Ei ) = dT + dT + dT γ Ei Ed 2Ed 2Ed Ec 2Ed

2 2 Ed σs (Ei ) (γ Ei ) 2 = − + γ Ei Ec − Ec . Ed + 2 γ Ei Ed 2 2

(2.121)

(2.122)

2.4 Displacement Rates

111

If we choose γ Ei ∼ Ec and neglecting terms in Ed or Ed2 gives:

σD (Ei ) ≈

γ Ei 4Ed

σs (Ei ) ,

(2.123)

and Eq. (2.2) becomes: Nγ 4Ed

∞

σs (Ei )Ei φ (Ei ) dEi γ E¯ i Φ, = N σs 4Ed

R=

E d /γ

(2.124) (2.125)

where E¯ i is an average neutron energy and Φ is the total neutron flux above energy Ed /γ , and the term in brackets is the number of displacements (Frenkel pairs) produced per neutron. The validity of assuming isotropic scattering and neglecting inelastic scattering is shown in Figs. 2.19 and 2.20. Essentially, both approximations are reasonable at energies below one to a few MeV.

Fig. 2.19. Recoil energy spectra from the elastic scattering of fast neutrons using data from ENDF/B files (after [22])

112

2 The Displacement of Atoms

Fig. 2.20. Displacement cross section for nickel showing the elastic and inelastic components (after [21])

Example 2.1. Neutron irradiation of iron. As an example, let us look at the damage caused by 0.5 MeV neutrons in Fe in a fast flux that may be representative of the core of a fast reactor: N = 0.85 ×1023 atoms/cm3

σs = 3 ×10−24 cm2 Φ = 1015 neutrons cm−2 s−1 γ Ei = 350 displaced atoms/neutron 4Ed R is 9 ×1016 displaced atoms per cm3 per second, or dividing R by N gives ∼ 10−6 dpa/s. This is equivalent to each atom being displaced from a normal lattice site once every 12 days. A second example can be worked for the displacement rate in the aluminum fuel plates in an MTR-type thermal neutron research reactor. In this case, we have: Ei ∼ 0.5 MeV N = 0.6 ×1023 atoms/cm3

σs = 3 ×10−24 cm2 Φ = 3 ×1013 neutrons cm−2 s−1

2.5 Correlation of Property Changes and Irradiation Dose

113

γ Ei = 690 displaced atoms/neutron 4Ed R is 4 ×1015 displaced atoms per cm3 per second, or dividing R by N gives ∼ 7 ×10−8 dpa/s, or about 2/yr. Note that even though the number of displacements per neutron is almost a factor of 2 higher in Al than in Fe, the damage rate is significantly lower because of the much lower fast flux in this type of reactor.

2.5 Correlation of Property Changes and Irradiation Dose The ultimate objective of the calculation of Rd is to provide a prediction of the extent of change of a particular property of the material under irradiation. The mechanical property may be yield strength, swelling, degree of embrittlement, etc. Recall in the Introduction that the determination of the number of displaced atoms was motivated by the inability of particle fluence to account for property changes (see Fig. I.1 in the Introduction). While an improvement over units of exposure such as neutron fluence, displacement rate alone cannot alone account for the macroscopic changes observed, and a semi-empirical method of correlating damage with macroscopic property changes has evolved known as the damage function method. In this method the atom displacement rate is replaced with the change in some macroscopic property after a time t of irradiation. The displacement cross section is replaced by the damage function for the particular mechanical property, Gi (E), hence: ΔPi j =

Gi (E)φ j (E,t) dE dt ,

(2.126)

where ΔPi j is the change in the property labeled by the index i, during an irradiation time of t and in a neutron flux where φ j (E,t) is the jth neutron differential spectrum. Assuming energy-time separability, φ j (E,t) = φ j (E)t, then Eq. (2.126) can be rewritten as: (k)

ΔPi j = t ·

(k)

Gi (E)φ j (E) dE ,

(2.127)

where the superscript refers to the kth cycle of iteration. The objective is to deduce a single function Gi (E) from a set of measured ΔPi (k) values. Given ΔPi j and φ j (E) as input along with an initial approximation of Gi (E) (0)

(k)

or Gi (E), a computer code is used to generate iterative solutions Gi (E). An appropriate solution is obtained when the standard deviation of the ratios of all (k) measured-to-calculated values ΔPi j /ΔPi j reaches a lower value that is consistent with experimental uncertainties. As it turns out, the resultant damage function is

114

2 The Displacement of Atoms

Fig. 2.21. (a) A 60 ksi yield strength damage function for 304 stainless steel irradiated and tested at 480 ◦C (after [23]). (b) Damage function for a 2.0 ×10−8 psi−1 ε¯ /σ¯ property change for stainless steel (after [24])

2.6 Displacements from Charged Particle Irradiation

115

Fig. 2.22. Dose dependence of swelling, resistivity and radiation-induced segregation

highly sensitive to the initial approximation as shown in Fig. 2.21. But note that since the shape of Gi (E) is the same as the displacement function, it is clear that they are related. However, this result tells us that we cannot fully understand radiation effects by only calculating the number of displaced atoms. We cannot treat radiation effects as a black box. Rather, in order to understand the effect of the damage on the properties of the material, we must understand the fate of these defects after they are formed. This realization is reinforced by the property dependence on dose shown in Fig. 2.22. Note that for the three property changes, resistivity, radiation-induced segregation and hardening, the functional dependence on dose is strikingly different between them. While property change certainly relates to displacement damage, the nature of the change is not uniform but varies considerably depending on the property measured. The next chapter explores the spatial and temporal distribution of radiation damage. But before we examine the damage zone in detail, let us complete our picture of the production of displacements by addressing the damage created by charged particles such as ions and electrons.

2.6 Displacements from Charged Particle Irradiation Displacements from charged particles differ from those due to neutrons because as they travel through the lattice, they lose energy via electronic excitation in addition to via elastic collisions. Figure 2.23 shows the trade-off in energy loss mechanism dominance with energy in the energy range of relevance for ion–solid interaction, and Fig. 2.24 shows the residual ion energy as a function of ion penetration depth. Note that electronic stopping will dominate at short depths, but elastic collisions

Fig. 2.23. Variation in nuclear and electronic stopping powers over the energy range of relevance to ion–solid interactions

116

2 The Displacement of Atoms Fig. 2.24. Residual range of an ion incident on a target and the regimes of electronic and nuclear stopping dominance

will dominate near the end of range. An expression for the number of displacements from a charged particle can be derived from the analysis of energy lost from the PKA by electronic excitation given in Sect. 2.2.3 and described by Eq. (2.40) through Eq. (2.49). Equation (2.44) describes the loss of energy to both atoms and electrons in the target by the PKA. We can revisit this analysis assuming that the particle we are tracking is the incident ion. As was done in Eq. (2.45), we can expand the terms for ν (T − εa ) and ν (T − εe ) in a Taylor series and truncate the series after the second term, giving: dν εa , dT dν ν (T − εe ) = ν (T ) − εe , dT

ν (T − εa ) = ν (T ) −

(2.128)

and the integrals involving the terms ν (T − εa ) and ν (T − εe ) can both be written in the general form: εmax 0

ν (T − ε )σ (T, ε ) dε = ν (T )

εmax 0

σ (T, ε ) dε −

= ν (T )σ (T ) −

dν dT

εmax

dν (T ) S(T ) . dT

0

εσ (T, ε ) dε

(2.129) Since in this treatment, the ion is the incoming projectile, we will re-write Eq. (2.129) using our established convention that the incoming particle is of energy Ei and it transfers energy T to the target atoms and electrons, and the maximum energy transfer is Tˆ : Tˆ

Tˆ

dν Tˆ ν (Ei − T )σ (Ei , T ) dT = ν (Ei ) σ (Ei, T ) dT − T σ (Ei , T ) dT dE 0 0 0 dν (Ei ) S(Ei ) , = ν (Ei )σ (Ei ) − (2.130) dE where Eq. (1.79) is used to transform the integral of the differential energy transfer cross section, σ (Ei , T ) to the total collision cross section σ (Ei ), and Eq. (1.129) is used to transform the integral of T σ (Ei , T ) into the stopping cross section S(Ei ).

2.6 Displacements from Charged Particle Irradiation

117

Applying the results of Eqs. (2.129) and (2.130) into Eq. (2.44) gives: dν (Ei ) =

dE S(Ei )

Tˆ 0

ν (T )σ (Ei , T ) dT .

(2.131)

Since we are concerned with the total number of displacements over the entire range of the ion rather than the specific number of displacements over a distance dx of the sample, we can integrate Eq. (2.131) over the entire range of ion energy loss to obtain the number of displacements resulting from an incident ion with initial energy Ei :

ν (Ei ) = =

Ei Tˆ dE

ν (T )σ (E , T ) dT

0

S(E )

0

dE , σd (E ) S(E )

Ei

Ed

(2.132)

and Tˆ Ed

ν (T )σ (E , T ) dT ≡ σd (E ) ,

(2.133)

where E = E (x) is the ion energy as a function of the traveled path length x as the ion travels down to zero energy. We can work a simple example using an approximation to the treatment given above. We are interested in the number of collisions made by an ion as it passes through a solid. We will take I as the ion flux in units of ions/cm2 and we can write the number of collisions per second in a volume element of unit cross sectional area and thickness dx which transfer energy in the range (T, dT ) to atoms of this element as: NI σ (E, T ) dx .

(2.134)

The number of collisions per unit volume per unit time which transfer energy in (T, dT ) at depth x is NI σ (E, T ) [collisions/cm3 s]. The number of displaced atoms for each collision that produces a PKA of energy T is ν (T ). Therefore, the production rate of displaced atoms at depth x is: Rd (x) = NI

γE Ed

σ (E, T )ν (T ) dT

[displacements/cm3 s] .

(2.135)

(Note that we have not accounted for the fact that I is a function of x (or E) and that I(x) = I0 .) E is a function of x since the ion slows down by loss of energy to the electrons of the target. The functional form of E(x) can be estimated using dE/ dx = kE 1/2 as: E(x) = [(Ei )1/2 − 1/2kx]2 ,

(2.136)

where Ei is the initial energy of the ion when it strikes the target. The number of dpa at a depth x is Rd (x)/NI. displaced atoms/atom/s is Rd (x)/N and the (ions/cm2 )

118

2 The Displacement of Atoms

We will assume that σ (E, T ) can be described by Rutherford scattering and using the Lindhard treatment for ν (T ) from the K–P model, and assuming ξ = 0.5 gives: γ Ei Rd 1 π Z12 Z22 ε 4 M + Mi 2 1 4Mi M 1 T = dT NI 4 M Ei (M + Mi )2 T 2 2Ed Ed 2 (2.137) π Z12 Z22 ε 4 Mi γ Ei dpa = . ln 4Ei Ed M Ed ion/cm2 Applying this result to 0.5 MeV protons in iron gives ∼ 10−18 dpa/(ions/cm2) at the surface. 20 MeV C+ ions incident on nickel produce ∼ 3 ×10−18 dpa/(ions/cm2) at the surface, but 50 times this amount at the damage peak. These values can be compared to the damage rate from 0.5 MeV neutrons in iron: Rd γ Ei = σs Nφ 4Ed (2.138) = 350 × 3 ×10−24 = 1 ×10−21

displacements . n/cm2 s

Comparing 0.5 MeV neutrons to 20 MeV C+ ions shows that over their range C+ ions produce 3000 times more displacements than do neutrons. Figure 2.25 com-

Fig. 2.25. Displacementdamage effectiveness for various energetic particles in nickel (after [25])

Nomenclature

119

pares the displacement rates as a function of penetration depth for ions of various mass and energy. As expected, for the same energy, ions of heavier mass deposit their energy over a shorter distance resulting in higher damage rates. Note that due to the large collision mean free path of a neutron as compared to an ion, the neutron damage energy is low and constant over distances of millimeters.

Nomenclature a a0 A A B B c D Ec Ech Efc Ed ED Ei Er Es Eγ Ei, Em Em E∗ Eeq f g G I¯ k m me M1 M2 N p, pe , pa Pch Pd Pf

Lattice constant Bohr radius of the hydrogen atom Atomic mass Pre-exponential constant in Born–Mayer relation, Eq. (1.47) Spacing between barrier atoms in crystal lattice Constant in exponent in Born–Mayer relation, Eq. (1.47) Speed of light Nearest neighbor spacing between atoms Cut-off energy; critical energy for focusing Critical energy for channeling Critical focusing energy Displacement energy Damage energy Projectile energy Critical energy for replacement collisions; relative kinetic energy Sublimation energy Gamma ray energy Incoming particle energy Kinetic energy of incoming particle in CM system Energy of neutron after (n, 2n) reaction Saddle point energy Energy of atom in equilibrium lattice site Focusing parameter Relative speed 1 − 2 Damage function Excitation-ionization level Force constant; constant in the electronic energy loss term, kE 1/2 Mass of incoming particle; 1/s Mass of the electron Mass of projectile Mass of target Atom number density Probability, refers to electron, refers to atom Channeling probability Displacement probability Focusing probability

120

2 The Displacement of Atoms

Q req rmax R Rch Rd S S, Se , Sn tc T Tˇ Tˆ T¯ T U V V (r) ν VCM 1 2 VCM Y z Z

Excitation energy of nucleus Equilibrium spacing between atoms Transverse amplitude of channeled atom Atomic radius Radius of channel Displacement rate [#/cm3 s] Exponent in the power law approximation Stopping power; electronic; nuclear Collision time Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy transferred to target atom after (n,2n) reaction Energy per atom in a crystal Energy per atom in a crystal Potential energy Specific volume of the atom Velocity of CM in lab system Velocity of projectile in lab system Velocity of target in lab system Velocity of center of mass Distance to atom barrier Impact parameter Atomic number

β ε εeq ε ε∗ φ,Φ γ η κ μ ν ν (T ) θ θc θch σ (Ei ) σ (Ei , T ) σD σs

Compressibility Secondary atom knock-on energy; unit charge Eq. (2.52) Energy of atom in a normal lattice site Reduced PKA energy Energy of atom at saddle point Neutron flux 4M1 M2 /(M1 + M2 )2 Energy lost to electronic excitation in the NRT model Displacement efficiency Reduced mass specific volume of an atom Displacement function Scattering angle in lab system Critical focusing angle Critical channeling angle Total atomic collision cross section Differential energy transfer cross section Displacement cross section Scattering cross section

Problems

σs j σ(n,2n) σγ τ ξ

121

Inelastic scattering cross section for the jth resonance Cross section for (n,2n) reactions Cross section for (n,γ ) reactions Period for oscillation for a channeled atom Damage energy efficiency, Eq. (2.50)

Problems 2.1 a) Using the simple K–P model and assuming only elastic, isotropic scattering, calculate the number of displacements per atom (dpa) in nickel subjected to a fast neutron (2 MeV) fluence of 1022 n/cm2 . b) Using the relativistic expression for the electron–atom energy transfer, calculate the minimum electron energy required to displace an atom in (i) Al and (ii) W. 2.2 In a (n, 2n) reaction, a second neutron can only be emitted if the residual excitation of the nucleus after emission of the first neutron exceeds the binding energy of a neutron in the mass M nuclide. The recoil energy after emission of the first neutron is taken to be the average value (cos φ = 0). Write an expression for the recoil energy following the second emission. 2.3 An 56 Fe nucleus undergoes an (n,γ ) reaction resulting in the release of a single 7 MeV gamma ray, on average. If a steel component is located in a reactor where the peak thermal flux is 1×1014 n/cm2 and the thermal/fast flux ratio is fast ≥ 1 MeV), determine the relative displacement rates by fast one (where Eave neutrons, recoil nuclei and gamma rays which undergo Compton scattering. Assume σ(n,γ ) ∼ 4b, σs ∼ 3b. 2.4 A slab of iron is exposed to a 20 MeV gamma source. a) What is the most probable interaction between the gamma and the electrons in the Fe? b) Assume the reaction you chose in part (a) occurs. Can this lead to the displacement of an Fe atom if the displacement energy is 40 eV? 2.5 A thermal neutron causes the following reaction 27

Al + n → 28 Al + γ .

The gamma energy is 1.1 keV. The gamma will interact with lattice electrons. What is the most probable event? For this event, what is the maximum energy transferred? Does the resultant electron have enough energy to displace an aluminum atom (assume the displacement energy is 25 eV). Can the recoil Al atom displace another aluminum atom? 2.6 The (n,γ ) reaction in 56 Fe releases a prompt gamma ray of Eγ = 7 MeV. a) What is the recoil energy of the 57 Fe product nucleus? b) Determine the number of displaced atoms per 57 Fe recoil assuming Ed = 40 eV. c) If the thermal component of the neutron flux in a fast reactor is 1013 n/cm2 s what is the damage production rate due to the (n,γ ) reaction in 56 Fe?

122

2.7

2.8

2.9

2.10

2.11

2.12

2.13

2 The Displacement of Atoms

d) If the fast flux is given by: φf (En ) = 1015 δ (En − 0.5), where En is in MeV, what is the damage production rate due to the fast flux in iron? Use the K–P displacement formula in (c) and (d). The scattering cross section for 0.5 MeV neutrons is 3 barns. Also, σa56 ∼ 2.5 barns for part (c). Assuming that atom–atom interactions can be treated as near head-on collisions, the appropriate potential function is then the Born–Mayer potential. Write an expression for the threshold energy for unassisted critical focusing along the [110] direction in fcc nickel in terms of the lattice constant, a. For iron (equilibrium phase for 400 ◦C), assuming a focusing collision occurs, how much does the closest approach (the allowed equivalent hard-sphere radius calculated using a Born–Mayer potential) change between a [100] collision chain and a [110] collision chain? a) Calculate the focusing energy of the 111 direction for gold under the condition of assisted focusing. b) Will focusing occur along the 111 direction in the absence of assisted focusing? Why? c) The experimental focusing energy of gold is 21,000 eV for the 111 direction. Compare your answer with this value. a) Determine the critical focusing energy for the 111, 110 and 100 directions in fcc copper and iron. b) Plot θc as a function of T < Ec for the 111 directions in Ni and Fe. Comment on similarities and differences. c) Do the same for the 110 direction of each. d) Repeat parts (a) and (b) using the inverse square potential, V (r) = A/r2 , where A = 1.25 eVnm2 . e) Over what energy range does focused replacement occur? How about focused energy packets only? For the focusing process as described in Problem 2.10, give a physical explanation of why the critical angle for focusing, θc , should depend on the projectile energy. A 30 keV ion enters a channel in the solid lattice and loses energy only by electronic excitation. Using the Lindhard stopping power formula Eq. (1.170), determine the distance traveled by the ion before it is dechanneled. The minimum channeling energy is 300 eV. Use k = 0.003NZ 2/3 eV1/2 /nm, where N is the atomic density of the metal in nm−3 . Show that when channeling is accounted for in the collision cascade, the average number of displaced atoms ν (T ) is:

ν (T ) − (T /2Ed )1−2p , where p is the probability that an atom with energy E being channeled is lost to the cascade. Assume that p = f (E), T Ed , and p 1. Assuming that all energy is lost by elastic collisions for 100 keV protons in nickel determine: a) The energy loss per unit length in the solid, dE/ dx b) The range in the solid.

References

123

2.14 A crystal of copper is bombarded with monoenergetic (2 MeV) neutrons. a) Calculate the mean atomic displacement rate (displacements/cm3 s) using the simple Kinchen–Pease model and the following data: Lattice parameter, Cu = 0.361 nm Atomic weight of Cu = 63.54 amu Displacement energy for Cu = 40 eV φ = 1013 n/cm2 s (2 MeV) σs = 0.5 ×10−24 cm2 (2 MeV) b) Repeat part (a) but instead of 2 MeV neutrons, use a monoenergetic thermal neutron beam where φth = φfast , σth = 3.78×10−24 cm2 and the recoil energy, ER ∼ 382 eV. c) What would be the effect on your answer to part (a) by including Lindhard’s damage energy function ξ (T )? d) How would your answer in part (a) be affected by assuming that the channeling probability is 1%, 5%, 10%? 2.15 For the 2 MeV neutron bombardment problem describe in Problem 2.14, how would you go about calculating the threshold energy for unassisted critical focusing along the [110] direction? 2.16 Assume that the copper target in Problem 2.14 was bombarded by a beam of 2 MeV He ions instead of a beam of 2 MeV neutrons. Calculate the displacement rate at the surface of the sample and compare to your result for Problem 2.14. 2.17 The same copper sample as in Problem 2.14 is bombarded with 500 keV Cu+ ions at a flux of 1015 cm−2 s−1 . Calculate: a) The displacement rate at the surface b) The location of the damage peak. Use a linear interpolation between the values of dE/ dx as given on the attached sheet.

References 1. 2. 3. 4. 5. 6.

7. 8. 9. 10.

Kinchin GH, Pease RS (1955) Rep Prog Phys 17:1 Seitz F (1949) Disc Faraday Soc 5:271 Bacon DJ, Deng HF, Gao F (1993) J Nucl Mater 205:84 King WE, Merkle KL, Meshii M (1983) J Nucl Mater 117:12–25 Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements. US DOE, Washington, DC ASTM E521 (1996) Standard Practice for Neutron Radiation Damage Simulation by Charged-Particle Irradiation. Annual Book of ASTM Standards, vol. 12.02. American Society for Testing and Materials, Philadelphia, PA Robinson MT (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge Snyder WS, Neufeld J (1955) Phys Rev 97(6):1636 Sanders JB (1967) Dissertation, University of Leiden Kohler W, Schilling W (1965) Nukleonik 7:389

124 11. 12. 13. 14. 15. 16.

17. 18. 19. 20. 21.

22. 23. 24. 25.

2 The Displacement of Atoms Sigmund P (1969) Appl Phys Lett 14(3):114 Lindhard J, Nielsen V, Scharff M (1968) Kgl Dan Vidnsk Selsk Mat Fyf Medd 36(10) Sigmund P (1969) Rad Eff 1:15–18 Erginsoy C, Vineyard GH, Englert A (1964) Phys Rev 133A:595 Lindhard J, Nielsen V, Scharff M, Thomsen PV (1963) Dan Vidnsk Selsk Mat Fyf Medd 33:1 Robinson MT (1972) The dependence of radiation effects on the primary recoil energy. In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 397 Norgett MJ, Robinson MT, Torrens IM (1975) Nucl Eng Des 33:50–54 Chadderton LT (1965) Radiation Damage in Crystals. Wiley, New York Brandt W (1968) Sci Amer 218:90 Datz S, Noggle TS, Moak CT (1965) Nucl Instr Meth 38:221 Doran DG (1971) Displacement Cross Sections for Stainless Steel and Tantalum Based on A Lindhard Model, USAEC Report, HEDL-TME-71-42. WADCO Corporation, Hanford Engineering Development Laboratory, April 1971 Robinson MT (1996) J Nucl Mater 216:1–28 Simmons RL, McElroy WN, Blackburn LD (1972) Nucl Technol 16:14 McElroy WN, Dahl RE, Gilbert ER (1970) Nucl Eng Des 14:319 Kulcinski GL, Brimhall JL, Kissinger HE (1972) Production of voids in pure metals by high-energy heavy-ion bombardment. In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 453

3 The Damage Cascade

3.1 Displacement Mean Free Path In our discussion of cascade development, no consideration was given to the spatial arrangement of displaced atoms. We assumed that every Frenkel pair created was preserved and that no annihilation occurred. However, the spatial arrangement of these Frenkel pairs is crucial in determining the number that survive annihilation or immobilization by clustering. In order to understand what the damaged region looks like, we need to know if the displacements are concentrated or distributed. A helpful tool in this regard is the mean free path for displacement collisions, i.e., collisions in which the energy transferred is greater than Ed . This will tell us how far apart the displacements occur and hence, the separation distance between Frenkel pairs. 1 By definition, the mean free path, λ = and the corresponding displacement Nσ cross section is:

σd (E) =

E Ed

σ (E, T ) dT .

(3.1)

This is the cross section for the transfer of energy in excess of Ed and is given in terms of the differential energy transfer cross section between lattice atoms. Note that σd has nothing to do with the projectile, be it a neutron or an ion, or the source of the damage in general. Using the equivalent hard-sphere model to evaluate σd gives:

σ (E) , γE but γ = 1, so substituting into Eq. (3.1) and integrating yields: E Ed σ (E) dT = σ (E) 1 − σd (E) = , E E Ed σ (E, T ) =

(3.2)

where σ (E) = 4π r2 is the total collision cross section between lattice atoms, so: Ed , (3.3) σd (E) = 4π r2 1 − E and r is the energy-dependent, equivalent hard-sphere radius, which, using the Born–Mayer potential gives:

2 2A Ed 2 σd (E) = π B ln 1− , (3.4) E E

126

3 The Damage Cascade

and the mean free path, λ becomes:

λ=

1 .

2 2A Ed 2 1− N π B ln E E

(3.5)

The mean free path and the total collision cross section are plotted in Fig. 3.1 for copper atoms in copper, and show that as the energy of the moving atom drops, the cross section increases slowly but the mean free path becomes very small at energies just above Ed . Note that the critical region (λ ∼ 0.3 – 1.0 nm), or the region in which every lattice atom in the path of the knock-on is displaced, lies in the energy range ∼ 50 – 100 eV. The mean free paths for primary recoil atoms of 300 keV and 1 MeV resulting from self-ion irradiations of Si, Cu and Au are shown in Fig. 3.2. Recall that T¯ = γ Ei ∼ 2Ei (for n-Cu interactions), where Ei is the neutron energy and A is the = 2 A atomic mass. Typically, Ei ∼ 0.5 MeV (for a thermal or fast reactor) and A ∼ 60 (stainless steel), giving T¯ ∼ 15 keV. So at large recoil energies, the displacements are well separated (∼ 100 nm at 15 keV), but as the recoil energy decreases, the spacing approaches the atomic spacing, at which point each atom along the recoil path is displaced.

3.2 Primary Recoil Spectrum The analysis of displacement mean free path gives us a first glimpse of what the spatial distribution of defects might look like. Brinkman [3] was the first to picture the cascade as a displacement spike with a high core density of vacancies surrounded by an interstitial shell (Fig. 3.3). Seeger [4] modified the picture to account for crystallinity such as focused energy packets (focusons), and long-range transport of mass by replacement collisions and channeling, and termed the vacancy core a depleted zone (Fig. 3.4). Two additional quantities are helpful in developing a picture of the distribution of damage energy. The first is the deposited energy depth distribution, FD (x), defined by: FD (x) dx = dE = NSn E(x) dx .

(3.6)

Using the nuclear stopping power and range given by the power law potential [5] results in a simple form for FD (x): FD (x) =

1 T (1 − x/R) 2m −1 , 2mR

(3.7)

where T is the PKA energy, R is the PKA range and m = 1/s where s is the power law exponent. If Nd (x) is the number of displacements per unit depth at a depth x, then using the modified K–P model or the NRT model (e.g., Eq. (2.53)) with κ = 0.8

3.2 Primary Recoil Spectrum

127

Fig. 3.1. Displacement mean free path and total collision cross section for copper atoms moving in copper (after [1])

Fig. 3.2. Mean free paths of primary recoil atoms of 300 keV and 1 MeV, self-ion irradiations of Si, Cu and Au (after [2])

128

3 The Damage Cascade

Fig. 3.3. Original version of the displacement spike as drawn by Brinkman (after [3])

Fig. 3.4. Revised version of Brinkman’s displacement spike as drawn by Seger (after [4]) accounting for crystallinity in the damage cascade

and with FD (x) replacing ED , we can write that: Nd (x) 0.8FD (x) = , φ 2Ed

(3.8)

and the displacement rate as a function of depth in units of dpa becomes: dpa(x) =

Nd (x) 0.4FD (x) = φ. N NEd

(3.9)

3.2 Primary Recoil Spectrum

129

The total dpa produced over the range of the recoil can be estimated by replacing FD (x) with the damage energy ED from Eq. (2.54) over the range of the recoil, R: dpa ∼ =

φ 0.4ED . NREd

(3.10)

The second important concept is the primary recoil spectrum. The density of recoil atoms with energies between T and T + dT that occur during irradiation is an important quantity in radiation damage. The recoil density depends on the projectile energy and mass and gives a measure of the density of displacement damage in the target. The density of recoils as a function of recoil energy is known as the primary recoil spectrum and is given as: P(Ei , T ) =

1 N

T Ed

σ (Ei , T ) dT ,

(3.11)

which is the fractional number of recoils between the minimum displacement energy Ed , and energy T , and N is the total number of primary recoils, and σ (Ei , T ) is the energy transfer cross section for a particle of energy Ei to create a recoil of energy T . The fraction of recoils is shown in Fig. 3.5 for 1 MeV projectiles of various mass incident on a copper target. Note that while higher mass projectiles produce more recoils at higher energy, the difference does not appear to be large. For defect production, it is not the number of recoils of a particular energy that is of greatest importance, rather it is the fraction of damage energy that are produced

Fig. 3.5. Integral primary recoil spectra for 1 MeV particles in copper. Curves plotted are the integral fractions of primary recoils between the threshold energy and energy, T from Eq. (3.11) (after [2])

130

3 The Damage Cascade

in recoils of a particular energy. This quantity is given by “weighting” the recoil spectra by the number of defects or the damage energy produced in each recoil: W (Ei , T ) =

1 ED (Ei )

T Ed

σ (Ei , T )ED (T ) dT ,

(3.12)

where ED (T ) is the damage energy created by a recoil of energy T : ED (Ei ) =

Tˆ Ec

σ (Ei , T )ED (T ) dT ,

(3.13)

and Tˆ = γ Ei . For the extremes of Coulomb and hard-sphere interactions, the differential energy-transfer cross sections are:

σCoul (Ei , T ) =

π M1 (Z1 Z2 ε 2 )2 , Ei T 2

(3.14)

and

σHS (Ei , T ) =

A . Ei

(3.15)

Ignoring electron excitations and allowing ED (T ) = T , and substituting Eqs. (3.14) and (3.15) into Eq. (3.12) gives the weighted average recoil spectra for each type of interaction: WCoul (T ) =

ln T − ln Tˇ , ln Tˆ − ln Tˇ

(3.16)

and WHS (T ) =

2 T 2 − Tˇ Tˆ 2

(3.17)

where Tˇ = Ed . Equations (3.16) and (3.17) are graphed in Fig. 3.6 for 1 MeV particle irradiations of copper. The Coulomb potential is a good approximation for proton irradiation while the hard-sphere potential is a good approximation for neutron irradiation. The Coulomb forces extend to infinity and slowly increase as the particle approaches the target. In a hard-sphere interaction, the particles and target do not “feel” each other until their separation reaches the hard-sphere radius at which point the repulsive force goes to infinity. A screened Coulomb is most appropriate for heavy ion irradiation. The result is that Coulomb interactions tend to create many PKAs with low energy while hard-sphere collisions create fewer PKAs but with higher energy. Note the large difference in W (T ) between the various types of irradiations in Fig. 3.6. While heavy ions come closer to reproducing the energy distribution of recoils of neutrons than do light ions, neither is accurate in the “tails” of the distribution. This does not mean that ions are poor simulations of radiation

3.3 Cascade Damage Energy and Cascade Volume

131

Fig. 3.6. Weighted recoil spectra for 1 MeV particles in copper, (after [2]). Curves representing protons and neutrons are calculated using Eqs. (3.14) and (3.15), respectively. W (T ) for other particles were calculated using Lindhard cross sections and include electronic excitation

damage, but it does mean that damage is produced differently and that this needs to be considered when assessing the microchemical and microstructural changes due to irradiation. Figure 3.7 illustrates the difference in the types of damage that is produced by different types of particles. Light ions such as electrons and protons will produce damage as isolated Frenkel pairs or in small clusters while heavy ions and neutrons produce damage in large clusters. For 1 MeV particle irradiation of nickel, half the recoils for protons are produced with energies less than ∼ 1 keV but with an average energy of 60 eV while the same number for Kr occurs at about 30 keV with an average energy of 5 keV. Recoils are weighted toward lower energies because of the screened Coulomb potential that controls the interactions of charged particles. For an unscreened Coulomb interaction, the probability of creating a recoil of energy T varies as 1/T 2 . Because neutrons interact as hard spheres, the probability of a creating a recoil of energy T is independent of recoil energy.

3.3 Cascade Damage Energy and Cascade Volume The energy density in a cascade of volume Vcas formed by an energetic projectile of energy Ei is given by [7]: ED Θ¯ D ∼ , = NVcas

(3.18)

132

3 The Damage Cascade

Fig. 3.7. Difference in damage morphology, displacement efficiency and average recoil energy for 1 MeV particles of different type incident on nickel (after [6])

where ED is the damage energy defined in Eq. (2.54) and N is the atom density of the target. To find the volume of the cascade requires knowledge of the depth distribution of the damage energy. Averback [2] showed that the volume of the cascade can be approximated by: Vcas =

4π ((δ ΔX)2 + 2(δ Y )2 )3/2 , 3

(3.19)

where (ΔX)2 and Y 2 are the longitudinal and transverse moments of the deposited damage energy distribution for an individual cascade, and δ is a contraction factor that accounts for the difference between an individual cascade and the average cascade determined by transport theory. While Eqs. (3.18) and (3.19) provide a description of the spatial extent of a cascade, other characteristics of the cascade are the temperature and temporal lifetime. The effective temperature of the cascade can be estimated by the relation: 3kB Tmax = Θ¯ D ,

(3.20)

where kB is Boltmann’s constant. The lifetime of the cascade or thermal spike can be estimated by solving the heat equation for the spread of energy from a point source in three dimensions. The variance in the temperature profile, R2 , is given by: R2 = 4Dτ ,

(3.21)

3.4 Computer Simulations of Radiation Damage

133

where τ is the cascade lifetime and D is the thermal diffusivity = κT /Cp , where κT is the thermal conductivity and Cp is the specific heat capacity. The cascade energy is then: 4 ED = π R3Ua N , 3

(3.22)

where Ua is the energy per atom. The cascade lifetime is determined by combining Eqs. (3.21) and (3.22) to solve for τ : 3ED 1 τ= . (3.23) 4D 4π NUa If we estimate Ua from the melting temperature of the target, then Ua ∼ 0.3 eV and D ∼ 1012 nm2 /s, then the lifetime of a 1 keV cascade is of the order 10−12 s, or a few lattice vibration periods.

3.4 Computer Simulations of Radiation Damage Analytical solutions to the space and time dependence of damage caused by an energetic particle incident on a target can take us only so far. And as we will see later, excellent instrumentation exists to observe defect clusters such as transmission electron microscopy, X-ray scattering, small angle neutron scattering and positron annihilation spectroscopy. But these instruments do not have the resolution to image individual defects and they cannot capture the temporal development of the cascade. To gain a better understanding of the spatial and temporal development of the cascade, we must turn to computer simulation. There are three principal techniques used to model the behavior of atoms in a displacement cascade; the binary collision approximation (BCA) method, the molecular dynamics (MD) method and the kinetic Monte Carlo (KMC) method [8]. Each will be briefly discussed. 3.4.1 Binary Collision Approximation (BCA) Method BCA simulations are useful for examining the collisional stages of high-energy cascades in statistically significant numbers. BCA simulations consider only the interactions between two colliding atoms at a time and in sequence [8]. The computation follows only the atoms having significant energies and are thus very efficient. The BCA approach provides a good approximation to the collision stage, since the neglected many-body interactions make little contribution to the atom trajectories at collision energies well above the atom displacement energy. At energies near or even less than the displacement energy, ballistic features of cascades such as replacement-collision sequences and focused-collision sequences (focusons) can be reasonably captured by BCA calculations. At primary recoil energies above approximately 20 keV, cascades may have more than one damage region. Because the mean free path between high-energy collisions of a recoil atom increases with energy,

134

3 The Damage Cascade

higher energy cascades will consist of multiple damage regions or subcascades that are well separated in space due to high-energy collisions. Channeling of primary or high-energy secondary recoils also contributes to subcascade formation when the channeled recoils lose energy and de-channel. There are two distinct types of BCA models. Those for crystalline targets are termed BC or binary crystal models and resemble MD models in that they assign all atoms to well-defined initial positions [9]. Models for materials without longrange order (amorphous solids) are termed MC or Monte Carlo models and use stochastic methods to locate target atoms and to determine collision parameters. The MC models are similar to transport theory models used in analytical theory to track neutron populations in a medium. An example of a BC model is the MARLOW code [10]. The program models crystalline targets with no restrictions on the crystal symmetry or on the chemical composition. All collision parameters are calculated from the particle positions. Several interatomic potentials are available for selection to describe atom collisions. Inelastic energy losses may be included in either local or non-local form, but the loses are limited to the velocity-proportional (E 1/2 ) range of kinetic energies. Figure 3.8 shows the spatial configuration of defects from an early computer simulation using the MARLOWE code for the case of a 200 keV cascade in copper. This is a very energetic cascade that would only be expected from extremely energetic neutrons such as are generated in a fusion reactor. The PKA is generated in the lower

Fig. 3.8. Collisional stage of a 200 keV cascade in copper simulated using the binary collision approximation in MARLOWE (after [8])

3.4 Computer Simulations of Radiation Damage

135

Fig. 3.9. Computer simulation of a displacement spike due to a 5 keV PKA in iron. All out-ofplane damage has been projected onto the 001 plane shown in the figure. (a) Recoil trajectories and (b) vacancies and interstitial atoms at the end of the collision cascade (0 K). The diagonal line in (b) shows the effect of channeling of a secondary knockon atom (after [11])

right hand corner (arrow) and proceeds to the left with a kinetic energy of 200 keV. The dark spheres are displaced atoms and the lighter spheres are vacant lattice sites. Note that the full cascade consists of several subcascades. A second example, shown in Fig. 3.9 shows how the cascade can become extended in space. The recoil trajectories and final configuration of interstitials and vacancies in bcc iron is shown after interaction with a 5 keV PKA at a temperature of 0 K [11]. All vacancies and interstitials within a sphere containing 30 lattice atom sites were assumed to recombine spontaneously. Note in Fig. 3.9a, that the secondary knock-on in the center of the spike undergoes channeling, making possible the extension of the cascade into the upper right half of the lattice shown in Fig. 3.9b. Essentially, all of the damage to the upper right of the diagonal is due to channeling of the secondary knock-on.

136

3 The Damage Cascade

TRIM [12] is another BCA code that uses Monte Carlo techniques to describe the trajectory of the incident particle and the damage created by that particle in amorphous solids and was discussed briefly in Chap. 1. TRIM uses a maximum impact parameter set by the density of the medium and a constant mean free path between collisions which is related to this. Stochastic methods are used to select the impact parameter for each collision and to determine the scattering plane. The barycentric scattering angle is determined by a “magic” formula, tested against published integral tables and represents the scattering from the ZBL “universal” potential. Inelastic energy losses are based on the effective charge formalism, using tables distributed with the code. Figure 3.10 shows a simulation of 3 MeV protons incident on a nickel target. Figure 3.10a shows the trajectories of the incident particles for 10,000 cases (MC runs), and Fig. 3.10b shows the ion concentration profile and the displacement rate profile as a function of depth. 3.4.2 Molecular Dynamics (MD) Method Molecular dynamics is the second major type of methodology used to describe collision cascades. MD is a computationally intensive method for modeling atomic systems on the appropriate scale for the simulation of displacement cascades and provides the most realistic description of atomic interactions in cascades [8]. Using realistic interatomic potentials and appropriate boundary conditions, the fate of all atoms in a volume containing the cascade can be described through the various stages of cascade development. The analytical interatomic potential functions must describe the force on an atom as a function of the distance between it and the other atoms in the system. It must account for both attractive and repulsive forces in order to obtain stable lattice configurations. In MD simulations, the total energy of the system of atoms being simulated is calculated by summing over all the atoms. The forces on the atoms are used to calculate acceleration according to F = ma, yielding the equations of motions for the atoms. The computer code solves these equations numerically over very small time steps, and then recalculates the forces at the end of the time step, to be applied in the calculations in the next time step. The process is repeated until the desired state is achieved. Time steps in MD simulation must be very small (5 – 10 ×10−15 s), so MD simulations are generally run for no more than 100 ps. As the initial primary kinetic energy E increases, larger and larger numerical crystallites are required to contain the event. The size of the crystallite is roughly proportional to E. The required computing time-scales roughly as E 2 . The demand on computing time limits the statistical capabilities of MD simulation. However, they provide a detailed view of the spatial extent of the damage process on an atomic level that is not afforded by other techniques. A cascade simulation begins by thermally equilibrating a block of atoms that constitutes the system to be studied. This process allows the determination of the lattice vibrations for the simulated temperature. Next, the cascade simulation is initiated by giving one of the atoms a specified amount of kinetic energy and an initial direction. Several cascades must be run in order to have results that can

3.4 Computer Simulations of Radiation Damage

137

Fig. 3.10. A 3 MeV proton incident on nickel as modeled by the TRIM code: (a) trajectory, (b) concentration profile and displacement profile

be used to represent the average behavior of the system at any energy and temperature. One such code used for MD simulations is the MOLDY code written by Finnis [13] and uses interatomic potentials developed by Finnis and Sinclair [13], and later modified by Calder and Bacon for cascade simulations [14]. The code only describes elastic collisions between atoms, and does not account for energy loss mechanisms such as electronic excitation and ionization. The energy given

138

3 The Damage Cascade

to the PKA in the MD simulation is that corresponding to the value of the displacement energy ED , given in Eq. (2.54). Stoller [15] conducted an MD simulation for iron and generated the cascade parameters shown in Table 3.1. Note that with increasing energy, the difference between the MD cascade energy and the PKA energy increases. Figure 3.11 shows typical point defect configurations from a 1 keV MD cascade simulation in iron at 100 K. Figure 3.11a shows the cascade at the point of peak disorder and Fig. 3.11b shows the cascade following in-cascade recombination. Note the sizable reduction in the residual damage between 0.18 ps and 9.5 ps. This result shows that the actual damage resulting from the PKA is much less than the total aggregate number of displacements calculated from the K–P or NRT models. While “still” images of the stages of the cascade are useful in understanding how the cascade develops, a much better appreciation is gained by viewing the temporal evolution of the cascade directly. This can be done by viewing Movie 3.1 via the website at www.sitemaker.umich.edu/was. This MD simulation shows the development of a cascade from a 200 keV recoil in iron at 100 K through to cascade quench at 21.6 ps. Note the extension of the cascade to the lower right hand corner that is probably do to a crystallographic effect involving channeling. Also note the striking difference in the defect density between the peak ballistic stage (∼ 0.7 ps) and the end of the quench at 21.6 ps.

3.4.3 Kinetic Monte Carlo (KMC) Method Our objective is to simulate the dynamical evolution of systems of atoms during and immediately following the displacement event. The most robust tool in this class of atomistic simulation methods is molecular dynamics. Integrating the classical equations of motion forward in time, the behavior of the system emerges naturally, requiring no intuition or further input from the user. A serious limitation, however, is that accurate integration requires time steps short enough (∼ 10−15 s) to resolve the atomic vibrations. Consequently, the total simulation time is typically limited to less than one nanosecond, while processes we wish to study (e.g., diffusion and annihilation of defects after a cascade event) often take place on much longer timescales. This is the “time-scale problem”. Kinetic Monte Carlo attempts to overcome this limitation by exploiting the fact that the long-time dynamics of this kind of system typically consists of diffusive jumps from state to state. Rather than following the trajectory through every vibrational period, these state-to-state transitions are treated directly. Given a set of rate constants connecting states of a system, KMC offers a way to propagate dynamically correct trajectories through the state space. If the rate catalog is constructed properly, the easily implemented KMC dynamics can give exact state-to-state evolution of the system, in the sense that it will be statistically indistinguishable from a long molecular dynamics simulation. KMC is the most powerful approach available for making dynamical predictions at the mesoscale without resorting to more dubious model assumptions. It can also be used to provide input to and/or verification for higher-level treatments such as rate theory models

3.4 Computer Simulations of Radiation Damage

139

Fig. 3.11. Typical point defect configurations from a 1 keV MD simulation in iron at 100 K at (a) the time of peak disorder (0.18 ps) and (b) following in-cascade recombination (9.5 ps). The larger, lighter spheres are interstitials, and the smaller, darker spheres are vacancies (after [15])

Table 3.1. Typical MD cascade parameters and required atom block sizes (from [15]) Cascade energy EMD ∼ ED (keV)

Corresponding PKA energy (keV)

NRT defects (NRT )

Atom block size (atoms)

0.1 0.2 0.5 1.0 2.0 5.0 10.0 20.0 50.0

0.116 0.236 0.605 1.24 2.54 6.61 13.7 28.8 61.3

1 2 5 10 20 50 100 200 400

3456 6750 6750 54,000 54,000 128,000 250,000 250,000 1,024,000

140

3 The Damage Cascade

Fig. 3.12. Time-scale for radiation damage evolution and the corresponding simulation methodologies

or finite-element simulations. Moreover, even in situations where a more accurate simulation would be feasible (e.g., using accelerated molecular dynamics or on-thefly kinetic Monte Carlo), the extreme efficiency of KMC makes it ideal for rapid scans over different conditions, for example, and for model studies. The result is that KMC can reach vastly longer time-scales, typically seconds and often well beyond. An example of the capability of KMC to capture processes on a larger timescale is given in Movie 3.2, which shows a KMC simulation of a 20 keV cascade in Fe–0.2Cu–0.6Si–0.7Ni–12.4Mn (similar to a pressure vessel steel) at 327 ◦C. The simulation shows the enrichment of Ni (green), Mn (black), Si (blue) and Cu (red) at cascade debris (vacancies in yellow) covering a time period out to several years, or many orders of magnitude longer than the cascade quench time. Note the pairing of Ni and Si and the accumulation of solute atoms at the vacancy clusters. Taken together, the MD and KMC methods cover the radiation time-scale as shown in Fig. 3.12. MD simulations are practical up to the ns range, and KMC simulations extend the range to the second [s] regime. Much occurs after this timescale and this is generally modeled using rate theory, which will be discussed in Chap. 5 and beyond.

3.5 Stages of Cascade Development The final state of the cascade is extremely important because the end of the cascade is the starting point for defect diffusion, agglomeration and destruction that forms the basis for the observable effects of irradiation to be covered in Part II of this text. Figure 3.13 shows another example in which a 2D cross section of a cascade is shown at times that correspond to the early stages of the cascade and near the final state. Here again, the damage state has relaxed to a very large degree between 2 ps (Fig. 3.13a) and 18 ps (Fig. 3.13b). Figure 3.14 shows the radial pair correlation function for the two times. The pair correlation function describes the separation of atoms and will appear as a series of spikes for crystalline solids (by virtue of their long-range order) and as a smoothly varying function for a liquid or amorphous solid (in which there is only nearest and second nearest neighbor correlation). As shown in the figure, the atom arrangement in the core of the displace-

3.5 Stages of Cascade Development

141

Fig. 3.13. MD simulation of a 30 keV displacement cascade in Cu at 300 K at 2 ps and 18 ps into the collision (calculations performed at the Barcelona Supercomputer center, courtesy of M. Catula and Tomas Diaz de la Rubia)

142

3 The Damage Cascade

Fig. 3.14. Pair correlation function for the collision cascades in Fig. 3.13, showing the amorphous-like character of the displacement cascade zone at 2 ps and the considerable degree of recovery by 18 ps (calculations performed at the Barcelona Supercomputer center, courtesy of M. Catula and Tomas Diaz de la Rubia)

ment spike at short times is similar to that of a liquid, while the final arrangement is recovering its crystalline configuration. Figure 3.15 shows that the mean square atomic displacement of atoms in the cascade also increases dramatically with time, indicating that the bulk of the aggregate movement of atoms in the displacement cascade occurs after the time to reach peak damage! Taken together, the results of Figs. 3.13–3.15 tell us that damage is annealing out with time. This annealing is occurring as the energy of the cascade is dropping. In fact, annealing occurs at the tail end of the period during which the cascade energy drops, called the quench stage. We now have a picture of how the cascade develops in time that we can describe. Cascades evolve in stages given as follows: 1. 2. 3. 4.

Collisional Thermal spike Quenching Annealing

In the collisional stage (1), the primary recoil atom initiates a cascade of displacive collisions that continues until no atom contains enough energy to create further displacements. At the end of this stage (lasting < 1 ps), the damage consists of energetic displaced atoms and vacant lattice sites. However, stable lattice defects have

3.6 Behavior of Defects within the Cascade

143

Fig. 3.15. Integrated diffusion coefficient as a function of distance from the center of the cascade at the end of the collisional phase, t = 0.12 ps (solid diamonds) and at the end of the cooling phase, t = 10 ps (open squares), for a 5 keV cascade in copper (after [16])

not yet had time to form. During the thermal spike stage (2), the collisional energy of the displaced atoms is shared among their neighboring atoms in the region of high deposited energy density. The development of the spike requires about 0.1 ps, and the spike may occupy several zones in which the energy is high enough so that the atoms resemble molten material. As energy is transferred to the surrounding atoms, the molten zones return to the condensed, or quenched stage (3), and thermodynamic equilibrium is established (∼ 10 ps). The quenching stage may take several ps and during this time, stable lattice defects form either as point defects or as defect clusters. But the total number of defects at this stage is much less than the number of atoms displaced in the collisional stage. The annealing stage involves further rearrangement and interaction of defects and occurs by thermally activated diffusion of mobile lattice defects. By definition, the annealing stage (4) lasts until all mobile defects escape the cascade region or another cascade occurs within it. Thus, the timescale extends from nanoseconds to months, depending on the temperature and the irradiation conditions. The annealing stage is the subject of the next part on Physical Effects of Radiation Damage (Part II) and is the link between the damage cascade and the observable effects of irradiation.

3.6 Behavior of Defects within the Cascade The actual number of defects that survive the displacement cascade and their spatial distribution in the solid will determine their effect on the irradiated microstructure. We define the displacement efficiency ξ , as the fraction of the “ballistically” produced Frenkel pairs (NRT dpa) that survive the cascade quench. MD simulation of the displacement cascade provides the recoil dependence of the displacement effi-

144

3 The Damage Cascade

Fig. 3.16. Dependence of the displacement efficiency on median PKA in copper. Open symbols refer to MD calculations and filled symbols refer to experimental measurements as the result of electron (•), ion (), fission fragment () and neutron () irradiation at low temperatures (after [17])

ciency in copper irradiated at low temperature (Fig. 3.16). The value of ξ increases rapidly from zero to > 1 at very low recoil energies. That ξ exceeds 1.0 is attributed to the inability of the modified K–P model to describe displacements in a polycrystalline material at recoil energies near the threshold displacement energy, Ed , due to the strong dependence of Ed on crystallographic orientation [17]. With increasing energy, ξ steadily decreases to a value of about 0.3 for 5 keV cascades in copper. The formation of multiple subcascades at high PKA energies (above ∼ 20 keV) causes ξ to remain nearly constant for PKA energies up to 500 keV. Comparing this plot to the recoil and weighted recoil spectra given in Figs. 3.5 and 3.6 shows that electrons and light ions with a low PKA energy will generate values of ξ close to 1, while heavy ions and neutrons that produce high PKA energies will result in ξ at the asymptotic value of 0.3. The displacement cascade efficiency, ξ is comprised of several components:

γi,v The isolated point defect fraction δi,v Clustered fraction including mobile defect clusters such as di-interstitials ζ Fraction initially in isolated or clustered form after the cascade quench that is annihilated during subsequent short term (> 10−11 s) intracascade thermal diffusion They are related as follows:

ξ = δi + γi + ζ = δv + γv + ζ .

(3.24)

3.6 Behavior of Defects within the Cascade

145

Fig. 3.17. Interdependence of isolated point defects, mobile defect clusters, and thermally evaporating defect clusters that contribute to the fraction of surviving defects that are “available” for radiation effects (after [17])

Figure 3.17 shows the history of defects born according to the NRT model as vacancies and interstitials. The fraction of defects that will be annihilated after the cascade quench by recombination events among defect clusters and point defects within the same cascade (intracascade recombination), ζ is about 0.07, for a displacement efficiency of 0.3. The clustered fraction, δ includes large, sessile clusters and small defect clusters that may be mobile at a given irradiation temperature and will be different for vacancies and interstitials. For a 5 keV cascade, δi is about 0.06 and δv is closer to 0.18. Some of these defects may be able to “evaporate” or escape the cluster and become “available” defects (Fig. 3.17). This leaves γ , the isolated point defect fraction as yet to be determined. These defects are available to migrate to sinks, to form clusters, to interact with existing clusters and to participate in the defect flow to grain boundaries that gives rise to radiation-induced segregation. Because of their potential to so strongly influence the irradiated microstructure, defects in this category, along with defects freed from clusters, make up the freely migrating defects (FMD). Recall that electrons and light ions produce a large fraction of their defects as isolated Frenkel pairs, thus increasing the likelihood that they remain as isolated defects rather than in clusters. Despite the equivalence in energy among the four particle types described in Fig. 3.7, the

146

3 The Damage Cascade

average energy transferred and the defect production efficiencies vary by almost two orders of magnitude! This is explained by the differences in the cascade morphology among the different particle types. Neutrons and heavy ions produce dense cascades that result in substantial recombination during the cooling or quenching phase. However, electrons are just capable of producing a few widely spaced Frenkel pairs (FP) that have a low probability of recombination. Protons produce small widely spaced cascades and many isolated FPs due to the Coulomb interaction and therefore, fall between the extremes in displacement efficiency defined by electrons and neutrons. The value of γ has been estimated to range from 0.01 to 0.10 depending on PKA energy and irradiation temperature, with higher temperatures resulting in the lower values. Because of the importance of this parameter, we will estimate the freely migrating defect fraction using an analytical treatment by Naundorf [18] that is based on two factors. The first is that energy transfer to atoms is only sufficient to create a single Frenkel pair. The second is that the Frenkel pair lies outside a recombination (interaction) radius so that the nearby FPs neither recombine nor cluster. The model follows each generation of the collision and calculates the fraction of all defects produced that remain free. According to Naundorf, the free single FPs are classified according to the generation i in which they were produced, i.e., the relative amount η1 is that amount that is produced by primary collisions (first generation), while η2 is the relative amount produced by secondary collisions (second generation). Thus the total number of free single FPs produced is:

η = ∑ ηi ,

(3.25)

i

where that produced by primary collisions is:

η1 = (βp /σd )

γE Ed

σ (Ei , T ) dT ,

(3.26)

and that produced by secondary collisions is:

η2 = (1/σd )

γE Ed

σ (Ei , T )[Z(T )βA (T )/σA (T )] dT

2.5Ed Ed

σ (T, T ) dT , (3.27)

where σ (Ei , T ) is the energy transfer cross section for an incident particle to a lattice atom and σ (T, T ) is the energy transfer cross section between like atoms in the solid, Z(T ) is the total number of secondary collisions produced above Ed by a PKA of energy T along its path. The primary displacement cross section for the incident ion, σp , is:

σp =

γE Ed

σ (Ei , T ) dT ,

(3.28)

and the total displacement cross section σd is given in the Kinchin–Pease model by:

σd =

γE Ed

σ (Ei , T )ν (T ) dT .

(3.29)

3.6 Behavior of Defects within the Cascade

147

The distance λ between two primary collisions is distributed according to an exponential law: W (λ ) = 1/λp exp(−λ /λp) ,

(3.30)

with the mean distance:

λp = Ω /σp ,

(3.31)

where Ω is the atomic volume. The condition that the distance between two consecutive collisions must be larger than an appropriate interaction radius, ri (so that FPs produced near each other neither recombine nor cluster) reduces the amount of all possible free single FPs by:

βp = exp(−ri /λp ) ,

(3.32)

and is illustrated in Fig. 3.18 [19]. The model provides the efficiency for the production of freely migrating defects. Results of this calculation are shown in Table 3.2 for several ions of varying mass and energy. Values of η range between 24% for proton irradiation to 3% for heavy ion (krypton) irradiation. Applying this model to our illustration in Fig. 3.7 yields the following values for η : MeV electrons: 3.4 MeV protons: 5.0 MeV Ni++ ions: Neutrons (fission spectrum):

1.0 0.2 0.04 0.02

These results can also be compared to those calculated by Rehn et al. [20] determined from analysis of experiments and are shown in Fig. 3.19. The data in this

Fig. 3.18. Illustration of the effect of the interaction radius on single Frenkel pair production

148

3 The Damage Cascade

Table 3.2. Calculated values for σp /σd and of the relative amounts ηcalc of FP production in nickel by different kinds of irradiations (Ed = 40 eV, ri = 0.7 nm) using Lindhard’s analytical differential collision cross section (from [18]) Irradiation

σp /σd (%)

ηcalc (%)

1 MeV H+ 2 MeV H+ 2 MeV Li+ 1.8 MeV Ne+ 300 keV Ni+ 3 MeV Ni+ 3.5 MeV Kr+ 2 keV O+

37.0 30.0 27.0 16.0 5.1 7.5 5.9 42.0

24.0 19.2 16.9 8.7 2.3 3.8 3.0 9.8

Fig. 3.19. Relative efficiency of freely migrating defect production for ions of various mass and energy (after [20])

figure are arbitrarily normalized to 1.0 for 1 MeV protons. This data along with the results just presented show that at low recoil energies, the fraction of defects that are freely migrating approaches 1.0 and as the recoil energy increases, that fraction drops to values in the range 0.02 to 0.05. Recent results [21], however, have shown that the low values of FMD efficiency for heavy ion or neutron irradiation cannot be explained by defect annihilation within the parent cascade (intracascade annihilation). In fact, cascade damage generates vacancy and interstitial clusters that act as annihilation sites for FMD,

3.6 Behavior of Defects within the Cascade

149

reducing the efficiency of FMD production. Thus, the cascade remnants result in an increase in the sink strength for point defects and along with recombination in the original cascade, account for the low FMD efficiency measured by experiment. While the NRT description of atom displacements provides an estimation of the number of Frenkel pairs produced by the PKA, it does not accurately describe atomic interactions in the thermal spike and hence, is inadequate for describing the true configuration of defects. MD simulations can be used for this purpose and have confirmed that defect production by displacement cascades is not as efficient as predicted by the NRT formula. In fact, ν is about 20 to 40% of NRT for cascades with energy greater than 1 – 2 keV. From analysis of MD results for several metals [22], the number of Frenkel pairs is found to depend on the kinetic energy of the PKA, T as:

νMD = AT n ,

(3.33)

where A and n are constants that are only weakly dependent on the metal and temperature. Figure 3.20 shows the dependence of νMD on T for various metals. Note that the behavior of Frenkel pair production is well represented by this function over a large damage energy range. Also note that the results all fall below the NRT value as shown by the solid line in the figure. The lower efficiency is likely the result of SIA production at the periphery of the disordered core dominating that at the end of focused collision chains such that the close proximity to the vacancies and the high kinetic energy of the core during the thermal spike assist in SIA-vacancy recombination. From the results shown in Fig. 3.20, there is no noticeable dependence on the crystal structure, as there are three fcc metals (Al, Ni, Cu), two hcp metals (Ti, Zr), one bcc metal (Fe) and one ordered L12 structure (Ni3 Al), and yet the magnitude of νFP is not separated along crystal structure lines. Second, there is a dependence on atomic mass of the metal as noted in the dependence of νMD and A on T . The dependence of n on atomic mass is weaker, though evident. The decrease in efficiency with atomic mass is likely due to the enhanced recombination due to thermal spike effects. As cascade energy increases, there is a tendency for cascades to break up into subcascades. Since one cascade produces fewer defects than two separate cascades of the same total energy, subcascade formation will increase the slope of the plots in Fig. 3.20. The transition to subcascades occurs at lower energy in lighter metals and may be the cause for the mass-dependence on efficiency. Note that n is only weakly dependent on mass. MD simulation has also been applied to the study of defect production in alloys [23, 24]. One might expect that the mass difference between solute atoms in an alloy will interrupt crystallographic processes such as focusing and channeling and result in the production of more Frenkel pairs as compared to the pure metal case. MD simulations in copper containing up to 15 at% gold in solution shows that the larger Au atoms decrease the length of focused displacement events in the ballistic phase and thereby enhance the intensity and lifetime of the disorder and temperature of the thermal spike. However, νFP was found to be independent on

150

3 The Damage Cascade

the alloy composition over a wide range of T . Similar studies conducted on Fe–Cu alloys substantiated these results. Movie 3.3 shows cascade formation and cooling in an Fe–10%Cr alloy in which the yellow balls are vacancies, the grey are iron interstitials and the green are chromium interstitials. In this simulation chromium is modeled as the larger solute, and after cooling, the remaining interstitial population is predominantly iron atoms as their distortion of the lattice is less than that from the oversized chromium atoms. The results shown in Fig. 3.20 are for MD calculations at or below a temperature of 100 K. Irradiation temperature has a strong effect on the evolution of radiation damage in metals because of its effect on the motion of defects and their stability as clusters. Irradiation temperature also has an effect on the formation of Frenkel pairs. Figure 3.21 shows the Frenkel pair production as a function of temperature in α -iron up through 900 K (627 ◦C) and for several values of PKA energy. Note that there is a small but consistent effect of temperature in that higher irradiation temperatures produce fewer Frenkel pairs. The lower Frenkel pair production is believed to be due to the increase in the lifetime of the thermal spike as Tirr increases, which allows for more defect motion before cooling and hence, more vacancy-interstitial recombination within the cascade region. A contributing factor may be the shorter length of the focused collision sequences (due to the higher kinetic energy of the atoms) that results in a reduction of the vacancy-interstitial separation distance.

Fig. 3.20. Number of Frenkel pairs produced as a function of damage energy, T for Cu, Fe, Ti, Zr and Ni3 Al at 100 K and for Al and Ni at 10 K (after [22])

3.6 Behavior of Defects within the Cascade

151

Fig. 3.21. Number of Frenkel pairs produced per cascade as a function of the PKA energy and irradiation temperature in α -iron (after [22])

In ordered alloys such as Ni3 Al (Fig. 3.20), the Frenkel pair production is similar to that in the pure metal (compare with Ni, for example). In addition to Frenkel pairs, anti-site defects or amorphization can occur in these systems. Anti-site defects consist of atoms of the wrong type occupying regular sites in the sublattice. These anti-site defects are observed to increase with T to the 1.25 power rather than to the 0.75 power as in the case of Frenkel pairs. If the amount of disorder is large enough, amorphization can occur. That the anti-site defects form in the molten core confirm that the thermal spike is important in the formation of these defects. The effect of increasing irradiation temperature on defect production in an ordered structure is to increase the number of anti-site defects, primarily due to the reduced length of focused collision sequences. We now have the description of the damage state that we need in order to begin to describe the development of the physical and mechanical effects of irradiation. The K–P/NRT models along with the energy transfer cross sections provide a means to calculate the number of displacements occurring in a solid from an incident particle of some mass and energy. The spatial, temporal and thermal descriptions of the resulting cascade provide us with a means to estimate the number of defects surviving the cascade quench phase, that are available to influence the microstructure at longer times. To this point, we have focused on developing both a physical and quantitative description of the state of the material at the end of the quench phase of the cascade that is completed within ∼ 10 ps of the initial collision event. From that point forward in time, we will be concerned with the development of the microstructure. This development will continue to occur for weeks, months and even

152

3 The Damage Cascade

years in a reactor core, spanning some 18 orders of magnitude in time, and constitutes the Physical Effects of Radiation Damage, which is the focus of Part II of this text.

Nomenclature A B Cp D Ea Ed ED Ei FD kB m M1 M2 N Nd P(Ei , T ) ri R s T Tˇ Tˆ T¯ Ua Vcas W (λ ) W (Ei , T ) ΔX Y Z Z(T )

βp δ δi,v

Atomic mass; pre-exponential constant in Born–Mayer relation, Eq. (1.47) Constant in exponent in Born–Mayer relation, Eq. (1.47) Specitic heat capacity Thermal diffusivity Energy per atom Displacement energy Damage energy Projectile energy Energy depth distribution Boltzmann’s constant 1/s Mass of projectile Mass of target Atom number density Number of displacements per unit depth Primary recoil spectrum Recombination radius Ion/atom range in the lattice Exponent in power law relationship Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy per atom Cascade volume Function for distance between primary collisions Weighted primary recoil spectrum Longitudinal moment of the cascade Transverse moment of the cascade Atomic number Fraction of secondary collisions produced above Ed by a PKA of energy T Reduction factor in FPs due to recombination within ri Cascade contraction factor Clustered fraction of vacancies and interstitials

Problems

ε φ γ γi,v η η1 η2 λ ν (T ) νFP Θ σ (E, T ) σD (E) σd σp τ ξ ζ

153

Unit charge Neutron flux 4M1 M2 /(M1 + M2 )2 Isolated point defect fraction Energy lost to electronic excitation in the NRT model; total # free FPs produced in cascade Fraction of defects produced by primary collisions Fraction of defects produced by secondary collisions Mean free path Displacement function Number of Frenkel pairs Cascade energy density Differential energy transfer cross section Displacement cross section for collisions between atoms Total displacement cross section Primary displacement cross section for incident ion Cascade lifetime Displacement efficiency Fraction of vacancies and interstitials initially clustered that are subsequently annihilated in the cascade

Problems 3.1 Plot the mean free path for Ni between the energies of 1 and 10,000 eV, making calculations at each decade. At what energy is the mean free path the smallest? Use Eq. (1.50) to determine the Born–Mayer constants and a value of 40 eV for Ed . 3.2 What is the implication of the difference in shape in the weighted recoil spectra for neutrons and protons in the morphology of the damage cascade? 3.3 For 1 MeV neutrons incident on nickel, determine a) The damage energy b) The effective cascade temperature c) The cascade lifetime using Ua ∼ 0.3 eV and D ∼ 1012 nm2 /s. 3.4 You would like to model displacement cascades. What is the appropriate modeling tool, kinetic Monte Carlo or molecular dynamics? Why? 3.5 Based on your expertise using SRIM, you decide to irradiate a steel sample (Fe–18Cr–9Ni) with nickel ions. You have the choice of examining the sample near the surface of the sample or near the damage peak. You are worried that all the implanted nickel ions will change the local chemistry of the sample. To mitigate this concern, should you look in the region closer to the sample surface or the damage peak? Why?

154

3 The Damage Cascade

References 1. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Service, Springfield, VA 2. Averback RS (1994) J Nucl Mater 216:49 3. Brinkman JA (1956) Amer J Phys 24:251 4. Seeger A (1958) On the theory of radiation damage and radiation hardening. In: Proceedings of the Second United Nations International Conference on the Peaceful Uses of Atomic Energy, Geneva, 1958, Vol. 6, p 250, United Nations, New York 5. Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge 6. Was GS, Allen TR (1994) Mater Character 32:239 7. Sigmund P (1981) Sputtering by ion bombardment: theoretical concepts. In: Behrisch R (ed) Sputtering by Particle Bombardment, Springer, Berlin Heidelberg New York, p 9 8. Heinisch HL (1996) J Metals Dec:38 9. Robinson MT (1994) J Nucl Mater 216:1 10. Robinson MT, Torrens IM (1974) Phys Rev B 9:5008 11. Beeler JR (1966) Phys Rev 150:470 12. Ziegler JF, Biersack JP, Littmark U (1996) The Stopping and Range of Ions in Solids. Pergamon, New York 13. Finnis MW, Sinclair JE (1984) Phil Mag A50:45–55; (1986) Erratum Phil Mag A53:161 14. Calder AF, Bacon DJ (1993) J Nucl Mater 207:25–45 15. Stoller RE (1996) J Metals Dec:23 16. Diaz de la Rubia T, Averback RS, Benedek R, King WE (1987) Phys Rev Lett 59(19):1930 17. Zinkle SJ, Singh BN (1993) J Nucl Mater 199:173 18. Naundorf V (1991) J Nucl Mater 182:254 19. Was GS, Allen TR (2007) In: Radiation Effects in Solids, Sickafus KE, Kotomin EA, Uberoage BP, eds, NATO Science Series, Springer 235:65–98 20. Rehn LE, Okamoto PR, Averback RS (1984) Phys Rev B 30(6):3073 21. Iwase A, Rehn LE, Baldo PM, Funk L (1996) J Nucl Mater 238:224–236 22. Bacon DJ, Gao F, Osetsky YuN (2000) J Nucl Mater 276:1–12 23. Deng HF, Bacon DJ (1996) Phys Rev B 54:11376 24. Calder AF, Bacon DJ (1997) In: Proceedings of Symposium on Microstructure Evolution During Irradiation, Vol. 439. Materials Research Society, Pittsburgh, PA, p 521

4 Point Defect Formation and Diffusion

The first step in understanding the effects of irradiation on materials is to understand, on the atomic level, the nature of radiation damage. In the previous chapters we developed a quantitative description of the process of displacing an atom from its lattice site by the transfer of kinetic energy from a high-energy particle. The recoiling lattice atom travels through the crystal, colliding with its neighbors and displacing these also from their sites. A cascade of atomic collisions is created by the original particle with the end result being a number of vacant lattice sites and an equal number of displaced atoms wedged into the interstices of the lattice. The basic defects (vacancies and interstitials) form the foundation for all observed effects of irradiation on the physical and mechanical properties of materials. Determination of the concentration and diffusion of these basic defects is the subject of this chapter.

4.1 Properties of Irradiation-Induced Defects Various types of defects exist in any crystalline lattice. These include: – – – –

Point defects (0D): vacancies and interstitials Line defects (1D): dislocation lines Planar defects (2D): dislocation loops Volume defects (3D): voids, bubbles, stacking fault tetrahedra

The most basic of these are point defects. Following [1], we will start with interstitials. 4.1.1 Interstitials An interstitial is an atom that is located in a position of a crystal that is not a regular lattice site. There are two broad classifications of interstitial sites in the various cubic crystal lattices: octahedral sites and tetrahedral sites, and these will be briefly reviewed. The fcc lattice is cubic with unit cell of length a (lattice constant) and with atoms located at the corners and the faces of the cube (Fig. 4.1). Each corner atom is shared by eight unit cells and each face atom is shared by two unit cells, so the number of atoms per unit cell is 8 corner atoms ×1/8 atom/unit cell + 6 face atoms ×1/2 atoms/unit cell = 4. Octahedral sites are interstitial positions that are

156

4 Point Defect Formation and Diffusion Fig. 4.1. Face-centered cubic (fcc) lattice unit cell

surrounded by an octahedron where the lattice atoms make up the six vertices of an octahedron. There are four octahedral sites per unit cell in the fcc lattice, the center of the unit cell and the edges. The center site is wholly within the unit cell, but the sites on the edges are each shared by four unit cells (Fig. 4.2a). So the total number of octahedral interstitial sites per unit cell is 1 + 12 edge sites ×1/4 site per unit cell = 4 sites. There are also tetrahedral interstitial sites in the fcc lattice in which the atom is located inside a tetrahedron formed by lattice atoms. These are located in side the corners of the unit cell (Fig. 4.2b). There are a total of 8 tetrahedral sites (one for each corner) in the fcc unit cell. In the bcc lattice, the atoms reside at the corners of the unit cell with one in the center of the cell for a total of two atoms per unit cell; 1 + 8 corner sites ×1/8 site/unit cell = 2 sites (Fig. 4.3). Octahedral interstitial sites are located on the faces and the edges of the unit cell giving 6 faces ×1/2 site per face +12 edges ×1/4 sites

Fig. 4.2. Interstitial positions in the fcc unit cell

4.1 Properties of Irradiation-Induced Defects

157

Fig. 4.3. Body-centered cubic (bcc) lattice unit cell

Fig. 4.4. Interstitial positions in the bcc unit cell

per edge = 6 sites per unit cell (Fig. 4.4a). Tetrahedral interstitial sites are located on the faces and in the corners of the faces. There are 6 faces × 4 locations per face × 1/2 sites/face = 12 tetrahedral sites (Fig. 4.4b). The hcp unit cell is not cubic but rather hexagonal and is defined by the c/a ratio where a is the length of a side of the regular hexagon and c is the height of the cell (Fig. 4.5). There are six atoms per unit cell in the hcp lattice; twelve on the corners shared by six cells (= 2) plus two on the faces shared by two cells (= 1) plus three inside the cell at a height of 1/2c (= 3). There are six octahedral sites per unit cell, all wholly contained within the unit cell (Fig. 4.6a). There are also six tetrahedral sites per unit cell, four wholly contained within the unit cell and six that are shared by each of three cells (Fig. 4.6b).

158

4 Point Defect Formation and Diffusion Fig. 4.5. Hexagonal close packed (hcp) unit cell

Fig. 4.6. Interstitial positions in the hcp unit cell

Our simple picture of interstitials is not a true physical picture because the stable configuration of self-interstitial atoms (SIA) in metals is the dumbbell or splitinterstitial configuration where two atoms are associated with or “share” a single lattice site. Since the atom cores repel each other, the atoms arrange themselves in the lowest energy orientation. This turns out to be with the dumbbell axis along the 100 direction for fcc metals, the 110 direction for bcc metals and the 0001 direction for hcp crystals (Fig. 4.7). To accommodate two atoms in one lattice site, atoms adjacent to the dumbbell are displaced slightly off their lattice positions which then perturbs neighboring atoms and so on. These displacements emanate from the defect, forming an elastic displacement field. The symmetry of the displacement field is reflected by the SIA configuration in the bcc lattice (Fig. 4.8). Consider a 100 dumbbell interstitial configuration in fcc aluminum. The separation distance of the two dumbbells is √ about 0.6a. The nearest neighbor spacing in the fcc lattice is along 110 and is (a/ 2). So the separation distance of a 100 dumbell is about 20% smaller than the nearest neighbor distance in the undistorted lattice. The four nearest neighbors to each dumbbell are displaced outwards by about 0.1a and the total relaxation volume is about 2Ω , where Ω is the atomic volume. The relaxation volume is determined by treating the crystal as an elastic continuum and inserting an atom as an interstitial (or removing one to create a vacancy) and

4.1 Properties of Irradiation-Induced Defects

Fig. 4.7. Configurations of SIAs in (a) fcc, (b) bcc and (c) hcp lattices

Fig. 4.8. Split interstitials in the bcc lattice

159

160

4 Point Defect Formation and Diffusion

Table 4.1. Numerical values, compiled from different sources for some quantities characterizing properties of radiation-induced point defects in metals (from [1]) Symbol Unit Interstitials i Relaxation volume Vrelax Formation energy Efi Equilibrium Ci (Tm ) concentration at Tm∗ i Migration energy Em Vacancies v Relaxation volume Vrelax Formation energy Efv Formation entropy Sfv Equilibrium Cv (Tm ) concentration at Tm∗ v Migration energy Em Activation energy QvSD for self-diffusion Frenkel pairs Formation energy

EfFP

Al

Atomic vol. 1.9 eV 3.2 – 10−18

Cu

Pt

Mo W

1.4 2.2 10−7

2.0 3.5 10−6

1.1

eV

0.12

0.12

0.06

Atomic vol. eV k –

0.05 −0.2 0.66 1.27 0.7 2.4 9 ×10−6 2 ×10−6

eV eV Qa

0.62 1.28

0.8 2.07

1.43 1.3 2.9 4.5

eV

3.9

3.5

5

−0.4 1.51 3.2

0.054

3.8 2 4 ×10−5 1.8 5.7

determining the amount of distortion resulting in the lattice. The high relaxation volumes due to SIAs cause large lattice distortions, which lead to strong interaction with other SIAs and with other lattice defects (dislocation, impurity atoms). The net effect of this elastic interaction is an attraction of mobile SIAs to these defects. Experimental values for the relaxation volume in several metals appear in Table 4.1. 4.1.2 Multiple Interstitials Multiple interstitials form by the agglomeration of mobile SIAs at elevated temperatures. Multiple interstitials have a high binding energy on the order of 1 eV. Since the energy needed to dissociate a SIA from a large cluster approaches the SIA formation energy (2 – 4 eV), SIA clusters are very stable against dissociation at low temperatures. Computer simulation predicts that the stable configuration of a di-interstitial in fcc metals is two parallel dumbbells on nearest neighbor sites (Fig. 4.9). The stable structure of tri-interstitials in fcc metals is predicted by computer simulation to be three orthogonal 100 dumbbells on nearest neighbor sites. The anticipated configuration of di-interstitials in the bcc lattice is two 110 dumbbells on nearest neighbor sites.

4.1 Properties of Irradiation-Induced Defects

161

Fig. 4.9. Di-interstitials in the (a) fcc lattice in stable, metastable and new stable positions, and (b) in the bcc lattice

4.1.3 Interstitial–Impurity Complexes Impurity atoms in metals are efficient traps for SIAs. Stable complexes consisting of undersized atoms and interstitials do not dissociate thermally below a temperature where vacancies become mobile. One possible configuration is the mixed dumbbell where one of the dumbbell atoms is replaced by the impurity atom (Fig. 4.10a). Binding energies are of the order of 0.5 – 1.0 eV. Weaker trapping is observed with oversized impurities (Fig. 4.10b). Interstitial–impurity complexes require only a small activation energy to reorient themselves by so-called cage motion. Shown in Fig. 4.10a, the impurity can jump between the indicated positions of the central octahedron, forming a new mixed dumbbell with the adjacent host atom. Since all of the mixed dumbbells have the impurity end toward the center of the cage, no long-range motion is associated with cage motion. The activation energy of the re-orientation jump in the cage is about 0.01 eV. Movies 4.1 and 4.2 show the behavior of iron and chromium in an Fe–10%Cr alloy following a displacement cascade as a function of the relative sizes of the solutes. In Movie 4.1, chromium is modeled as an oversized solute and in Movie 4.2, chromium is undersized. Note the difference in the interstitial clusters following the cascade cooling period. The undersize Cr (Movie 4.2) undergoes stronger trapping by the iron interstitials than in the case of oversize Cr (Movie 4.1), resulting is a greater number of small interstitial clusters containing Cr.

162

4 Point Defect Formation and Diffusion

Fig. 4.10. (a) Mixed dumbbell configuration in the fcc lattice formed by an undersized impurity and an atom of the host lattice. The vertices of the octahedron are the other locations of the impurity as it makes a dumbbell with the other “face” atoms in the unit cell. (b) Trapping of an interstitial to make a dumbbell with an oversized impurity in the fcc lattice

4.1.4 Vacancies The vacancy, or missing lattice atom, is the simplest point defect in metal lattices. All calculations and computer simulations show that the single vacancy structure is a missing lattice atom with the nearest neighbors relaxing inward toward the vacancy. SIAs have a high formation energy (> 2.0 eV), a large relaxation volume (∼ 2 Ω) and a low migration energy (< 0.15 eV) leading to a high mobility. Vacancies, on the other hand, have low formation energies (< 2 eV), low relaxation volume (0.1 – 0.5 Ω) and high migration energy (> 0.5 eV) and are therefore much less mobile than SIAs (Table 4.1). Further, the strain field of vacancies is isotropic in cubic metals making them hard to investigate. 4.1.5 Multiple Vacancies Multiple vacancies have small binding energies compared to interstitial clusters (0.1 eV) but are often observed in irradiated metals. The configuration of multiple vacancy clusters is shown for the fcc lattice in Fig. 4.11a, and for the bcc lattice in Fig. 4.11b. The migration energy of di-vacancies is less than for single vacancies (0.9 eV vs. 1.32 eV for Ni) but increases with increasing cluster size. It appears that since the tetra-vacancy can only migrate by dissociation, it is the first stable nucleus for further clustering. 4.1.6 Solute–Defect and Impurity–Defect Clusters Vacancies can bind to oversize solute or oversize impurity atoms in order to lower the overall free energy of the solid. Estimates of the binding energy of a vacancy to an oversize solute in the fcc lattice range from 0.2 to 1.0 eV [2]. Hence, these solutes can act as efficient traps for vacancies in the lattice.

4.1 Properties of Irradiation-Induced Defects

Fig. 4.11. Configurations of multiple vacancies in the (a) fcc lattice, and (b) bcc lattice

163

164

4 Point Defect Formation and Diffusion

4.2 Thermodynamics of Point Defect Formation Even in the absence of irradiation, a crystal cannot exist at finite a temperature in a state of absolute perfection. Statistically, there is a finite probability that sufficient energy will be concentrated, by local fluctuations, to form a defect in the crystal lattice. For most purposes, it is fair to assume that the volume of the crystal is constant, for which the Helmholtz free energy function applies. Following [3], if the system is at constant pressure then: F∼ = G = U + pV − T S = H − T S ,

(4.1)

where U is the internal energy, H is the total enthalpy of the N atoms comprising the system. S represents the disorder (entropy) in the system which can be characterized by: S = k ln w ,

(4.2)

where w is the number of possible different configurations of atoms and k is Boltzmann’s constant. Suppose that a crystal has n defects with N available sites. The increase in free energy is: ΔGf = nΔHf − T ΔS ,

(4.3)

where ΔHf is the increase in enthalpy brought about by the introduction (formation) of the defect and ΔS is the change in total entropy, determined as follows. For one defect, there are N available sites and hence N possible configurations. For n defects, there are N for the first, (N − 1) for the second, (N − 2) for the third, etc., up to (N − n + 1) for the nth. This leads to N(N − 1)(N − 2) . . . (N − n + 1) configurations in all. But because these are not all distinct and defects are indistinguishable, the number above allows for n! ways of distributing N defects among n sites. Hence, the number of possible different configurations is: w=

N(N − 1)(N − 2) . . . (N − n + 1) , n!

(4.4)

w=

N! . n!(N − n)!

(4.5)

or

The mixing entropy is then: ΔSmix = k [ln N! − lnn! − ln(N − n)!] .

(4.6)

Using Stirling’s approximation of ln x! x ln x for large x gives: ΔSmix = k ln w ∼ = [N ln N − n lnn − (N − n) ln(N − n)] .

(4.7)

4.2 Thermodynamics of Point Defect Formation

165

In addition to ΔSmix there is a contribution to Δ S from the vibrational disorder of the presence of the defects. According to the Einstein model of lattice motion, the atoms are represented as 3N independent linear harmonic oscillators and the associated entropy is: kT Sf = 3k ln , (4.8) h¯ νE where νE is the natural frequency of the oscillator and h¯ is Planck’s constant. If each defect changes the vibration frequency of z neighbors to νr , the entropy is:

kT kT νE Sf = 3kz ln = 3kz ln + ln , (4.9) h¯ νr h¯ νE νr and for n defects, the total change in entropy due to vibrational disorder is: νE n(Sf − zSf ) = ΔSf = 3nkz ln . (4.10) νr Taking both contributions to the entropy change and inserting them into the free energy equation gives: 3z νE ΔGf = nΔHf − kT N ln N − n lnn − (N − n) ln(n − N) + n ln . (4.11) νr In equilibrium, n will be such that it satisfies dΔGf / dn = 0 giving: ΔHf N − n νE 3z . = ln kT n νr

(4.12)

Assuming n N and letting n/N = C (concentration): C= Writing

νE νr νE νr

3z

−ΔHf exp kT

.

(4.13)

3z in terms of entropy gives the familiar equation:

ΔSf −ΔHf −ΔGf n exp = exp . C = = exp N k kT kt For vacancies we have: v Sf −Efv Cv = exp exp , k kT

(4.14)

(4.15)

166

4 Point Defect Formation and Diffusion

and for interstitials: i S −Efi Ci = exp f exp , k kT

(4.16)

where Efv = ΔHfv and Efi = ΔHfi and Efv , Efi are the formation energies for the respective defect type, and ΔSfv = Sfv , ΔSfi = Sfi . In metals, typical values for Efv are ∼ 1 eV, and for Efi ∼ 4 eV. Hence the formation of vacancies requires considerably less energy than the formation of interstitials (see Table 4.1) and so at thermal equilibrium, Cv Ci . Let us look at an example.

Example 4.1. Calculate the equilibrium concentration of vacancies and interstitials in aluminum at room temperature and 10 ◦C below the melting point. a) RT 20 ◦C or 293 K From Table 4.1, we have: Efv ∼ = 0.66 eV i∼ E = 3.2 eV f

Sfv ∼ 0.7 k Sfi ∼ 8 k ,

and inserting into Eqs. (4.14) and (4.15) yields: Cv = exp (Sfv /k) exp (−Efv /kT ) ∼ 1.6 ×10−11

Ci = exp Sfi /k exp −Efi /kT ∼ 5.0 ×10−51 . b) At 10 ◦C below Tm or 650 ◦C (923 K) Eqs. (4.15) and (4.16) yield: Cv = exp (Sfv /k) exp (−Efv /kT ) ∼ 5.0 ×10−4

Ci = exp Sfi /k exp −Efi /kT ∼ 9.8 ×10−15 .

Besides doing an experiment, how do we go about obtaining an estimate for Efv ? Suppose we create a small cavity in a rigid crystal that has a volume Ω = 4/3π ra3 equal to the volume occupied by one atom, where Ω is the atom volume and ra is the atom radius. Since we must conserve volume, we spread the material from the cavity uniformly over the surface of a crystal. If the crystal is a sphere, we have: R = R + ΔR .

(4.17)

Since the crystal is a rigid medium and volume is conserved: 4π R2ΔR = 4/3π ra3 ,

(4.18)

4.3 Diffusion of Point Defects

167

and if the crystal is large compared to the size of the atom, then R ra and ΔR R and: ΔR = ra3 /3R2 .

(4.19)

If Efv is the difference in surface energy of the crystal with and without a cavity and σ is the surface energy per unit area, then: Efv = 4π ra2 σ + 4πγ (R + ΔR)2 − 4π R2σ

(4.20)

∼ 4πσ (ra2 + 2RΔR)2 , where the first two terms on the right hand side of the equation are the energies associated with the inner and outer surfaces after formation of the vacancy and the last term is the energy of the surface of the crystal before formation of the vacancy, and the ΔR2 term has been neglected. Substituting for ΔR from Eq. (4.19) gives: 2 ra3 v 2 Ef = 4πσ ra + 3R 2 ra 2 = 4πσ ra 1 + , (4.21) 3R and since ra R, we have: Efv ∼ 4πσ ra2 .

(4.22)

In most metals, σ ∼ 10 eV/nm2 and ra ∼ 0.15 nm, so Efv ∼ 2 eV. If we treat the crystal as an elastic continuum, we get a different expression for Efv : Efv = 4π ra2 σ − 12π ra

σ2 σ2 + 6π ra , μ μ

(4.23)

where the first term is the surface energy of the cavity, the second term is the reduction in surface energy due to contraction of the surface by the surface tension, and the third term is the elastic energy stored in the solid, μ is the shear modulus of the crystal, and Efv ∼ 1 eV. Note that an interstitial will cause a displacement that is greater than ra , resulting in a greater formation energy as we have seen already.

4.3 Diffusion of Point Defects Atoms in a lattice are in a constant state of motion due to thermal vibration, and this means that point defects in the lattice are also in motion. The random nature of thermal vibration gives rise to random walk of the atoms via the defects that are in thermal equilibrium with their surroundings, known as self-diffusion. If foreign atoms are present in a pure metal, their diffusion is known as heterodiffusion.

168

4 Point Defect Formation and Diffusion

Self-diffusion arises when a local concentration gradient of defects appears in the crystal, driving atoms to move in the direction that eliminates the gradient. Diffusion is driven by forces other than the concentration gradient, such as stress or strain, electric fields, temperature, etc. Diffusion in a polycrystal is a complex mechanism due to the presence of grain boundaries, internal surfaces, dislocations, etc. We will follow the analysis in [4] by starting with diffusion in a single crystal and then expanding our treatment to include the polycrystalline case later on. 4.3.1 Macroscopic Description of Diffusion Diffusion is governed by two fundamental laws derived by Fick in 1880. They apply to any state of matter due to their general character regarding macroscopic diffusion processes. The first law is a relationship between the flux, J, and the concentration gradient of the diffusing specie: J = −D∇C ,

(4.24)

where D is the diffusion coefficient and ∇C is the composition gradient. For diffusion in one dimension: ∂C . (4.25) J = −D ∂x The minus sign indicates that diffusion takes place in the direction of decreasing concentration of the diffusing specie. D is generally given in units of cm2 /s or m2 /s and for solids between 20 and 1500 ◦C, 10−20 cm2 /s < D < 10−4 cm2 /s. Fick’s second law gives a relation between the concentration gradient and the rate of change of concentration caused by diffusion at a given point in the system:

∂C = −∇ · J = −∇ · D∇C , ∂t which, in one dimension simplifies to ∂C ∂ ∂C =− D . ∂t ∂x ∂x

(4.26)

If D is not a function of the concentration, then we can write Eq. (4.26) as:

∂C = −D∇2C ∂t (4.27) ∂ 2C = −D 2 . ∂x Equations (4.26) or (4.27) can be solved for certain limiting conditions enabling D to be determined on the basis of various measurements. While Fick’s laws provide a description of diffusion on the macroscopic scale, we would like to understand diffusion on the microscopic level as well. Diffusion occurs by several possible mechanisms depending on the nature of the diffusing specie and the host lattice. We will examine these mechanisms and then derive a description of diffusion on the microscopic level.

4.3 Diffusion of Point Defects

169

4.3.2 Mechanisms of Diffusion To obtain a theoretical description of diffusion, we first consider the elementary act of a jump of an atom from one stable position to another in the lattice. There are several mechanisms of lattice diffusion, some requiring the presence of defects, others not. The following types [5] can be distinguished. Exchange and ring mechanisms: The exchange mechanism (Fig. 4.12) consists of the exchange of lattice positions involving two atoms located in adjacent crystal sites. It does not require the presence of defects, and it is highly improbable in close packed crystals since it requires considerable deformation and hence, an enormous activation energy. The ring mechanism (Fig. 4.13) is less energy intensive but requires the coordinated movement of three to five atoms. Since the probability of this is low and the energy required is still high, both the exchange and ring mechanisms are unimportant in crystals containing defects. Vacancy mechanism: This is the simplest mechanism of diffusion and occurs in metals and alloys (Fig. 4.14). Diffusion occurs by the jump of an atom from its lattice site to a vacant site. For an atom to move by this mechanism the presence of a neighboring vacancy is required. Since movement of the vacancy is opposite that of the atom, vacancy-type diffusion is regarded as either a movement of the atom

Fig. 4.12. Exchange mechanism of diffusion

Fig. 4.13. Ring mechanism of diffusion

170

4 Point Defect Formation and Diffusion Fig. 4.14. Vacancy mechanism of diffusion

or the equivalent movement of the vacancy. However, as we will see, the diffusion coefficient for vacancy diffusion is not equal to that for atom diffusion. Interstitial mechanism: This mechanism involves the movement of an atom from one interstitial position to another (Fig. 4.15). It requires considerable energy in order to push its way through the barrier atoms separating the interstitial sites in the crystal (recall the role of barrier atoms in our calculation of displacement energy in Chap. 2). In reality, this mechanism only occurs when the diffusing specie is of an atom type that is smaller than the host lattice atoms. Interstitialcy mechanism: This mechanism involves the displacement of nearby lattice atoms to an interstitial site and generally occurs when atom diameters are comparable. There are two variants of this mechanism: the collinear variant in which displaced atoms move along a straight line (Fig. 4.16a) and the non-collinear variant in which the displaced atom moves to the interstitial position at an angle to the direction of movement of the displacing atom (Fig. 4.16b). Dumbbell interstitial mechanism: This process involves the symmetrical placement of an interstitial and a lattice atom about a single lattice site such that they share the lattice site. Figure 4.17 shows a 2D schematic of the sharing of a single lattice site by two atoms. Recall from our discussion in Sect. 4.1, that the dumbbell is a very stable configuration for the interstitial and that there are preferred directions for the dumbbell that depend on the lattice, and minimize the energy.

Fig. 4.15. Interstitial mechanism of diffusion

4.3 Diffusion of Point Defects

171

Fig. 4.16. Interstitialcy mechanism of diffusion, (a) collinear variant, (b) non-collinear variant

Fig. 4.17. Dumbbell interstitial mechanism of diffusion

Crowding (crowdion) mechanism: This mechanism occurs when an atom is added to a lattice plane but it does not reside in an interstitial position. To accommodate the atom, lattice atoms over, perhaps, 10 lattice constants are all shifted with respect to their lattice sites. The configuration can be thought of as a dumbbell spread over 10 atoms along a row, rather than two (Fig. 4.18). Actually, we have already seen a crowdion in our discussion of focusing collisions. Re-examine Fig. 3.4 and you will see a crowdion emanating from the displacement spike. This configuration is not a stable configuration and exists only temporarily as the energy for the knock-on atoms is expended. Despite the numerous mechanism for diffusion of atoms in a solid, diffusion usually occurs by either the vacancy or interstitialcy mechanisms. Ultimately, we want to obtain a mathematical relation between the macroscopic parameters for diffusion (i.e., the self-diffusion coefficient) and the elementary acts of defect jumps represented by the coefficients of diffusion for defects, or the microscopic process. We will assume that the self-diffusion process consists of a completely random walk of defects, i.e., there is no correlation between successive jumps of the defects. Although this is reasonable for defect diffusion, it is not strictly true for atom diffusion.

172

4 Point Defect Formation and Diffusion Fig. 4.18. Crowdion mechanism of diffusion

As mentioned earlier, jumps of defects and hence, atoms, are due to thermal vibrations of very high frequency. The Debye frequency is ∼ 1013 s−1 . The frequency of atom jumps is orders of magnitude lower, ∼ 108 s−1 at say, 700 ◦C. This means that once every 105 vibrations, a thermal fluctuation is large enough for an atom to overcome the energy barrier separating it from the next stable position. Let us take a closer look at the jumping process. 4.3.3 Microscopic Description of Diffusion Suppose that at time zero, a single impurity atom is placed in a position in a crystal which is designated as the origin. The atom proceeds to jump from one site to another in a completely random manner. Each jump is of distance λ , but since the medium is assumed to be isotropic, each jump is arbitrary and independent of previous jumps. After a time t, the displacement, r, of the particle from the origin is measured. If the experiment is repeated several times, r will not be the same because of the stochastic nature of the process. Rather, the displacements will be distributed according to a function Pt (r) where Pt d 3 r is the probability of finding the atom in a volume element d 3 r a distance r from the origin after time t. The quantity that best describes the extent of migration is the mean square displacement, r2 , which is given by the second moment of the distribution: r2 =

all space

r2 Pt (r)d 3 r = 4π

∞ 0

r4 Pt (r)dr .

(4.28)

We will first compute r2 without knowledge of Pt (r). If the atom makes Γ jumps per unit time, the time interval t corresponds to a number of n jumps given by: n = Γt .

(4.29)

Each jump is represented by a vector λ i , where the subscript, i, refers to the jump number. The vectors are all of the same length, λi , but of random direction. The

4.3 Diffusion of Point Defects

173

Fig. 4.19. Random jump of a defect in an isotropic solid

position of the diffusing atom after n jumps (Fig. 4.19) is the vector sum of the λ i or: r = λ 1 + λ 2 + .λ 3 . . . + λ n .

(4.30)

The magnitude of the square of the displacement is obtained by taking the scalar product of r with itself: r2 = r · r = (λ 1 + λ 2 + .λ 3 . . . + λ n ) · (λ 1 + λ 2 + .λ 3 . . . + λ n ) .

(4.31)

The scalar product of two sums is equivalent to squaring the sums, giving: n

n−1 n

i=1

i=1 j =i

r2 = ∑ λ i · λ i + 2 ∑ ∑ λ i · λ j .

(4.32)

The first term is equal to nλ 2 and the second term can be rewritten as:

λ i · λ j = λ 2 cos θi j ,

(4.33)

and n−1 n

r2 = nλ 2 + 2λ 2 ∑ ∑ cos θi j ,

(4.34)

i−1 j =i

or

r = nλ 2

2

2 n−1 n 1 + ∑ ∑ cos θi j n i=1 j =i

.

(4.35)

The mean square displacement is obtained by averaging r2 over a large number of experiments. The term cos θi j can range from −1 to 1, and by nature of the random hopping process, the average value of cos θi j for any i j combination is zero. Hence, the last term disappears and: r 2 = nλ 2 ,

(4.36)

r2 = λ 2 Γ t .

(4.37)

or

Equation (4.37) relates the mean square displacement to the microscopic properties of jump distance and jump frequency. Now, we wish to compute r2 from a macroscopic viewpoint.

174

4 Point Defect Formation and Diffusion

At t = 0, N impurity atoms are introduced into a restricted region of a host crystal. As a consequence of diffusion (random hopping), the N atoms spread out from the origin in a manner described by C(r,t) which is obtained by solving Fick’s second law (assuming D is not a function of concentration): 1 ∂ ∂C ∂C =D 2 r2 , (4.38) ∂t r ∂r ∂r with initial condition C(r, 0) = 0, for r = 0. Since the N atoms remain in the crystal, C(r,t) is subject to the constraint: ∞ 0

4π r2C(r,t) dr = N ,

(4.39)

with boundary condition that the concentration drops to 0 at infinity, C(∞,t) = 0. The solution to Eq. (4.38) subject to the initial and boundary conditions becomes: exp −r2 /4Dt . (4.40) C(r,t) = N (4π Dt)3/2 The probability of finding the single atom in a spherical shell between r and r + dr after time t, is equivalent (in the macroscopic diffusion description of the problem) to the fraction of the N atoms located in the same volume element after time t. Pr (r) and C(r,t) are related by: C(r,t) exp −r2 /4Dt = . (4.41) Pt (r) = N (4π Dt)3/2 The mean square displacement is: r 2 = 4π

∞ 0

r4 Pt (r) dr

4π = (4π Dt)3/2

∞ 0

r4 exp −r2 /4Dt ,

(4.42)

or r2 = 6Dt .

(4.43)

Comparing to r2 = λ 2Γ t from our microscopic solution Eq. (4.37), we have: D = 1/6λ 2Γ ,

(4.44)

which is the Einstein formula and is the link between the microscopic diffusion parameters λ and Γ , and the macroscopic diffusion parameter, D. 4.3.4 Jump Frequency, Γ We define Γ as the total number of jumps per second for an atom. Therefore, in a time increment δ t, we expect Γ δ t jumps. The quantity Γ δ t is proportional to z,

4.3 Diffusion of Point Defects

175

the number of nearest neighbors (sites), pv , the probability that a given neighboring site is vacant, and ω , the frequency with which an atom jumps to a particular site. Thus, the frequency with which an atom jumps to any neighboring equilibrium site, Γ , is the product of the jump frequency to a single site, ω , the number of nearest neighbor sites, z, and the probability that one site is vacant, pv , or:

Γ = zpv ω ,

(4.45)

Dva = 1/6zλ 2 pv ω .

(4.46)

and

where we have properly included the subscript a and superscript v to indicate that this is the diffusion coefficient for atom diffusion via vacancies. Also note that the jump distance λ is related to the lattice constant by λ = Aa, where the coefficient, A, depends on the diffusion mechanism and the crystal structure. The terms 1/6zA2 are often lumped together into a single parameter, α , such that: Dva = α a2 pv ω ,

(4.47)

and if vacancy motion is random, then pv = Nv and: Dva = α a2 Nv ω .

(4.48)

Let us look at an example of how to determine α for a specific diffusion process and crystal structure.

Example 4.2. Vacancy diffusion in the bcc and fcc lattices In the case of the vacancy mechanism of diffusion in a bcc structure, each atom√has eight nearest neighbors (z = 8). The jump distance is related to a by A = 23 , and hence, α = 1. For the simple interstitial diffusion mechanism in a bcc lattice, z = 4 and A = 1/2 giving α = 1/6. For the fcc lattice, z = 12 and A = √12 , giving α = 1. For interstitials in the fcc lattice, z = 12 and A = 1/2 and α = 1/2. Before continuing, it is instructive to point out the difference between vacancy diffusion and atom diffusion via a vacancy mechanism (vacancy self-diffusion). In determining the components of Γ , we noted that Γ depends on the probability, pv , that a neighboring lattice site is vacant. This is a necessary condition for an atom jump via a vacancy. However, if we are following the migration of the vacancy, then Γ depends on the probability that a neighboring lattice site to the vacancy is filled by an atom. Since in all but the most extreme cases, this probability is ∼ 1, and the equation for vacancy diffusion is given as follows: Dv = α a 2 ω , and differs from that for vacancy self-diffusion by the factor Nv .

(4.49)

176

4 Point Defect Formation and Diffusion

4.3.5 Jump Frequency, ω In calculating ω we will ignore detailed atomic movements and instead deal in terms of “activated complexes” or regions containing an atom midway between two equilibrium sites (Fig. 4.20). The number of atoms diffusing per second is then obtained by multiplying the number of activated complexes (nm ) by the average velocity of the atoms moving through this barrier (ν¯ ) divided by the width of this barrier (δ ). The jump frequency is then:

ω=

Nm ν¯ , δ

(4.50)

where Nm is the mole fraction of activated complexes. The work done in moving an atom across this barrier is equal to the change in Gibbs free energy for the region, ΔGm : ΔGm = ΔHm − T ΔSm .

(4.51)

Using ΔGm , the equilibrium mole fraction of atoms in the region of the saddle point in Fig. 4.20, Nm can be calculated in the same way we calculated Nv . Instead of mixing vacancies to raise the free energy by ΔGv per mole, we are mixing complexes to raise the free energy an amount ΔGm per mole. The ideal entropy of mixing is the same for vacancies as for complexes so, at equilibrium, nm out of N atoms will be in the neighborhood of the saddle point at any instant and: −ΔHm + T ΔSm nm −ΔGm = Nm = exp = exp . N kT kT

(4.52)

Nm ν¯ and ν¯ /δ is the frequency (call it ν ) at which atoms at From Eq. (4.50), ω = δ the saddle point jump to the new site. Thus Nm ν out of N atoms will jump from one

Fig. 4.20. Passage of the “activated complex” from one stable position, through a saddle point, to another stable position

4.3 Diffusion of Point Defects

site to a given site per second, and the average jump frequency is: −ΔGm ΔSm nm ν −ΔHm = ω = ν exp = ν exp exp N kT k kT Sm −Em = ν exp exp , k kT

177

(4.53)

where ν is the Debye frequency (∼ 1013 s−1 ) and Em = ΔHm and Sm = ΔSm . 4.3.6 Equations for D We are now in a position to write the expressions for the diffusion coefficients for the motion of the defects, and of the atoms by way of the defects: 1. The vacancy diffusion coefficient is given by: Dv = α a 2 ω where

ω = ν exp

−ΔGvm kT

= ν exp

then

Sv Dv = α a ω = α a ν exp m k 2

2

v Sm k

exp

v −Em exp kT

v −Em kT

,

(4.54)

2. The vacancy self-diffusion coefficient is the product of the vacancy diffusion coefficient and the probability that the nearest neighbor site is vacant, Nv : Dva = α a2 Nv ω , where NV = exp

−ΔGvf kT

giving:

Dva = α a2 ν exp

= exp

Sfv k

exp

Efv kT

,

v Sfv + Svm −Efv − Em exp . k kT

(4.55)

3. The interstitial diffusion coefficient is: Di = α a 2 ω , or

Di = α a2 ν exp

i Sm k

exp

i −Em kT

.

(4.56)

178

4 Point Defect Formation and Diffusion

4. The interstitial self-diffusion coefficient is the interstitial diffusion coefficient times the probability that a neighboring site contains an interstitial, Ni : Dia = α a2 Ni ω , where

Ni = exp

−ΔGif kT

giving

= exp

Sfi k

exp

−Efi kT

,

i i Sfi + Sm −Efi + −Em exp . (4.57) k kT The diffusion coefficients are all different in detail, but similar in form as they consist of two factors; a constant that is independent of temperature and an exponential of temperature containing an energy term. All equations for D can be rewritten in the form: (4.58) D = D0 exp(−Q/kT ) , where D0 = α a2 ν is the temperature independent term and Q is the activation energy. For vacancy diffusion we have: v Qv = E m , (4.59) and for vacancy self-diffusion we have: v Qva = Efv + Em . (4.60) For interstitials we have: i and Qi = Em , (4.61) and for interstitial self-diffusion we have: i Qia = Efi + Em . (4.62) It follows that the activation energy for diffusion of atoms in a crystal depends on both the energy of formation of defects and the energy required for their migration in the periodic field of the crystal lattice. Experiments can be conducted to confirm the temperature dependence of D and also the values of Q. The terms in the pre-exponential factor for the various diffusion mechanisms are provided in Table 4.2 for the fcc and bcc lattices. Dia = α a2 ν exp

Example 4.3. Determination of Dva and Dia for fcc copper at 500 ◦C For copper: Efv = 1.27 eV ,

Efi = 2.2 eV

v = 0.8 eV , Em

i Em = 0.12 eV

Sfv = 2.4 k ,

Sfi

v and Si . and we neglect Sm m

∼0

4.3 Diffusion of Point Defects

179

√ For the fcc lattice, z = 12, A = 1/ 2, and a ∼ 3 nm, giving: −0.8 2 Dv = α a ν exp kT −6 2 ∼ cm /s 5 ×10 = −0.12 2 Di = α a ν exp kT −2 2 ∼ = 7 ×10 cm /s Dva = α a2 ν exp

2.4k −1.27 − 0.8 exp k kT

∼ = 3 ×10−13 cm2 /s −2.2 − 0.12 i 2 Da = α a ν exp kT −16 2 ∼ 3 ×10 cm /s = Note that while Di /Dv ∼ 104 due to the smaller migration energy for interstitials than for vacancies, but Dia /Dva ∼ 10−3 because of the very high interstitial formation energy compared to that for vacancies. Plots of the diffusion coefficients are shown in Fig. 4.21. Note that the vacancy diffusion coefficient is larger than the vacancy self-diffusion coefficient and has a smaller slope.

Table 4.2. Parameters in the expression for the diffusion coefficient, D = α a2 N ω , where α = 1/6zA2 for the various diffusion mechanisms in the fcc and bcc lattices Diffusion mechanism

z

A

α

N

D

Vacancy Vacancy self-diffusion Interstitial Interstitial self-diffusion

12 12 12 12

fcc√ 1/√2 1/ 2 1/2 1/2

1 1 1/2 1/2

1 Nv 1 Ni

a2 ω a2 Nv ω 1/2a2 ω 1/2a2 Ni ω

Vacancy Vacancy self-diffusion Interstitial Interstitial self-diffusion

8 8 4 4

bcc √ √3/2 3/2 1/2 1/2

1 1 1/6 1/6

1 Nv 1 Ni

a2 ω a2 Nv ω a2 ω 1/6a2 Ni ω

180

4 Point Defect Formation and Diffusion Fig. 4.21. Comparison of plots of ln D vs. 1/T for vacancy diffusion and vacancy selfdiffusion

The behavior of self-interstitial atoms in bcc iron at 323 ◦C is illustrated in Movie 4.3. In this movie, the green balls are the interstitials and the red ball is the vacant lattice site, and together they form a SIA dumbbell in which the two green atoms share a single lattice site. The SIA originates as a 110 split-dumbbell interstitial and then rotates into a 111 interstitial and moves in one-dimension through the 111 crowdion saddle position. Movie 4.4 shows a di-SIA consisting of two parallel 111 split-dumbbells that migrates along the 111 direction and also rotates to different 111-type orientations.

4.4 Correlated Diffusion Earlier we assumed that irrespective of the kinds of defects present in a crystal lattice, successive jumps of atoms are completely random or uncorrelated. This means that after n jumps, all possible directions for the (n + 1)th jump are equally probable. This is true for vacancies or interstitials since all structural elements surrounding them are at all times identical. Since the vibrational frequency of a lattice atom is several orders of magnitude greater than the jump frequency, equilibrium in the region surrounding the defect is rapidly established between successive jumps and the next jump occurs with no effect of the previous jump on its direction. But this does not always hold true for atom diffusion as described in [5] and in the following. If we consider the case of a radioactive tracer to track atom diffusion, a tracer will make a jump if a vacancy is in its immediate vicinity. The second jump is uncorrelated with the first if the probability of the second jump is the same for all directions. However, the tracer arrives from a position that is vacant at the time of its arrival. Hence, when it is “preparing” for the next jump, the chance that the position from which it has arrived is unoccupied is greater than for any other position around the atom. The two jumps are correlated since the probability of the tracer returning to its former position is higher than for making a jump in any other direction. In

4.4 Correlated Diffusion

181

other words, the tracer has a greater tendency to move in the direction from which it came than in the direction it is headed, or from Eq. (4.35), cos θ 2 < 0. Since jumps in the direction from which it came are most probable, the tracer will have traveled a shorter (net) distance than that traveled by the vacancy. Therefore, the self-diffusion coefficient of the tracer (which is a measure of the rate of this process) is smaller than that of the atoms constituting the lattice, since the self-diffusion of the tracer is a correlated random walk whereas the movement of the vacancies and consequently of the atoms constituting the lattice are not correlated. The correlation effect is absent in the simple interstitial mechanism, but there is correlation of motion by the interstitialcy mechanism. In both the vacancy and the interstitialcy mechanisms, Dtracer < Dlattice and: f=

Dtracer , Dlattice

(4.63)

and f is known as the Haven coefficient and is a measure of the degree to which diffusion is random. Recall our earlier discussion of the measurement of the square of the displacement by random walk given by Eq. (4.35): 2 n−1 n 2 2 r = nλ 1 + ∑ ∑ cos θi j , n i=1 j =i where the mean square displacement is obtained by averaging over all values of cos θi j . In this expression the term in brackets is f and the value of f for random walk is 1 since the average over all cos θi j is 0. But when there is correlation between successive jumps, f is = 1. For the vacancy mechanism of diffusion of a tracer in a regular lattice [5]: fv =

1 + cos θ , 1 − cos θ

(4.64)

and for interstitial diffusion, fi = 1 + cos θ .

(4.65)

Since in both cases, cos θ < 0, then f < 1. 1−P , where P is the probability of a jump A simpler treatment of fv is that fv = 1+P of a tracer to a neighboring vacancy, and 1 − P is the probability that a neighboring vacancy will move away as a result of jumps of lattice atoms. To a first approximation, P is equal to the reciprocal of the number of nearest lattice sites, z, around the tracer. Therefore: f=

1 − 1/z z − 1 = . 1 + 1/z z + 1

(4.66)

182

4 Point Defect Formation and Diffusion

For the fcc lattice: f=

1 − 1/12 12 − 1 = = 0.85 . 1 + 1/12 12 + 1

For the bcc lattice: f=

1 − 1/8 8 − 1 = = 0.78 . 1 + 1/8 8 + 1

For the simple cubic (sc) lattice: f=

1 − 1/6 6 − 1 = = 0.71 . 1 + 1/6 6 + 1

So, in our microscopic description of the diffusion coefficient D, Eq. (4.44), we account for correlated diffusion by including the correlation coefficient: D = 1/6 f λ 2Γ = f α a2 ω .

(4.67)

As an aside, the true correlation coefficient, f , actually consists of two terms, f and f such that f = f f . The quantity f was described in the previous section (as f ) and f is related to the difference between the distances traveled during the elementary act by the tracer atom and the defect: f =

λtracer , λdefect

(4.68)

In the case of a vacancy, f = 1 since λtracer = λvacancy , or the distance traveled by the tracer and the defect are equal in one jump. The same is true for the simple interstitial mechanism. But in the case of the interstitialcy mechanism, the tracer moves from an interstitial position to a lattice site (or vice versa). In both cases, it travels a distance λtracer . However, the passage of a lattice atom from an interstitial position to a lattice site is equivalent to the appearance of an identical atom displaced from the lattice site in a neighboring interstitial position. Therefore, the jump of a lattice atom from the interstitial position to a lattice site requires (for the collinear case) a displacement of the lattice atom by a distance 2λtracer , or f = λtracer /2λtracer = 0.5. For the noncollinear case, f = λtracer /1.6λtracer = 2/3. Table 4.3 summarizes the correlation coefficient for various diffusion mechanisms in the common crystal lattices.

4.5 Diffusion in Multicomponent Systems Our discussion on diffusion so far has applied only to pure or single-component systems. We have not accounted for multiple components such as impurities in a pure metal and alloys. Diffusion in these systems was treated in experiments conducted by Smigelskas and Kirkendall in 1947 [6] and analyzed by Darken in 1948 [7]. The

4.5 Diffusion in Multicomponent Systems

183

Table 4.3. Correlation coefficients for the most common diffusion mechanisms in the various crystal lattices (from [5]) Crystal lattice

Diffusion mechanism

Correlation factor

Simple cubic

Vacancy Interstitial Collinear Non-collinear Vacancy Interstitial Collinear Non-collinear Vacancy Vacancy

0.65311

Face-centered cubic

Body-centered cubic Hexagonal close packed

0.80000 0.96970 0.72722 0.66666 0.72740 0.72722 0.78121

result is that the diffusion coefficients of the two components in a binary (A–B) system can be expressed as: D˜ = DA NA + DB NB ,

(4.69)

where DA,B are the intrinsic diffusion coefficients and are functions of composition, and D˜ is the interdiffusion coefficient. Since the partial diffusion coefficients depend on the alloy composition, D˜ is a complex, non-linear function of concentration. However, in the case of dilute solutions (NB → 0, NA → 1), the interdiffusion coefficient is approximately equal to the partial diffusion coefficient of the solute. The significance of this result can be appreciated by a brief review of the elegance and implications of the experiment. In Kirkendall’s experiment, molybdenum wires were wound around a block of brass (70Cu–30Zn) which was then plated with a thick coating of copper. The molybdenum wires are insoluble in copper and act as inert markers to locate the original interface. When the assembly is heated in a furnace, the wire markers on opposite sides of the brass moved toward each other, indicating that more material has left the brass than entered it, implying that the diffusion coefficient of zinc is greater than that of copper. The vacancy mechanism is the only diffusion mechanism that can account for marker motion. If zinc diffuses by a vacancy mechanism, then the flux of zinc atoms in one direction must equal the flux of vacancies in the opposite direction and the number of zinc atoms leaving the brass is balanced by an equal number of vacancies entering the brass. But the vacancies are absorbed by internal sinks, so the result is that the volume of the brass diminishes and the markers move closer together. The concept of a flux of atoms giving rise to a flux of defects will be explored in depth in Chap. 6 on Radiation-Induced Segregation, which occurs by the inverse Kirkendall effect.

184

4 Point Defect Formation and Diffusion

4.6 Diffusion along High Diffusivity Paths Metals and alloys used as structural engineering materials are polycrystals and are thus, inhomogeneous, as they contain grain boundaries, dislocations, internal interfaces due to precipitates or second phases, etc. To understand diffusion in these systems, we must discuss the effect of these linear, planar and area defects on the diffusion process. The primary difference between mono- and polycrystals is that the latter consists of aggregates of crystals oriented (generally) at random. This latter type of structure rarely shows anisotropy of diffusion. The important difference is that linear and planar defects represent high diffusivity paths along which diffusion can occur much faster than via point defects (bulk diffusion). Grain boundaries are important high diffusivity paths since the atom packing density is lower. There exist several models of grain boundary diffusion, and all assume that the boundary has of width, δ ∼ 0.3 –0.5 nm. One model that is based on the dislocation model of grain boundaries deserves special attention. In this model, the grain boundary is regarded as a number of edge dislocations. The dislocation density (#/unit length) increases with increasing misorientation angle θ , between two grains in contact (Fig. 4.22). From the figure: d sin

b θ = . 2 2

(4.70)

Hence, the distance between neighboring dislocations decreases with increasing misorientation angle. A low angle grain boundary consisting of many edge dislocations can be regarded as a row of parallel channels in which packing of atoms is loosest. In this region, the strain is high and the packing of atoms is loose, and the diffusion coefficient will be the highest along the dislocation lines (cores). According to this model, diffusion along grain boundaries should be anisotropic, and depend on the angle θ . The grain boundary described as a slab of uniform thickness δ and diffusion coefficient Dgb , can also be viewed as a planar array of pipes of radius p and spacing d. Grain boundary diffusion is related to diffusion along dislocation cores (also known as pipe diffusion), described by Dp , by the following relation: Dgb δ = Dp (π p2 /d) ,

(4.71)

and substituting for d from Eq. (4.70) gives: 2 2 sin θ /2 = Dp π p b Dp π p 2 θ ∼ . = b

(4.72)

The dislocation model of the grain boundary shown in Fig. 4.22 is expanded in Fig. 4.23 to show that the extra half planes of atoms can be regarded as edge dislocations. In fact, the rate of diffusion along the grain boundary increases with increasing misorientation angle, θ , and reaches a maximum at θ = 45◦ (Fig. 4.24).

4.6 Diffusion along High Diffusivity Paths

185

Fig. 4.22. Dislocation model of a small angle grain boundary and the geometrical relationship between the angle of tilt, θ , the Burgers vector, b, and the spacing between the dislocations, d

Fig. 4.23. Expanded view of the dislocation model of the grain boundary shown in Fig. 4.22

186

4 Point Defect Formation and Diffusion

Fig. 4.24. Effect of grain boundary misorientation angle on the diffusion of atoms along grain boundaries (after [5])

At angles greater than 45◦ , the dislocation model of grain boundaries breaks down since the distance between dislocations, d, would have to be smaller than the lattice constant. This result also indicates that there should be a relationship between the mean ¯ in a polycrystalline material and the grain value of the diffusion coefficient, D, size, d, since as the grain size decreases, the grain boundary area per unit volume increases. Therefore, D¯ should increase with decreasing grain size as shown in Fig. 4.25. We can write the diffusion coefficient of a solid in which diffusion occurs by bulk diffusion (vacancy mechanism) and grain boundary diffusion as: −Qgb −Qva v ¯ + Dgb exp , (4.73) D = Da exp kT kT where Dva and Qva refer to vacancy self-diffusion and Dgb and Qgb refer to grain boundary diffusion. In most metals, Qva ∼ 2Qgb , so at low temperature, grain boundary diffusion dominates and at high temperature, diffusion is dominated by bulk, or volume diffusion (Fig. 4.25). Pipe diffusion along dislocation cores can also influence low temperature lattice diffusion and the total diffusion coefficient can be estimated simply by: D¯ = f Dp + (1 − f )Dva ,

(4.74)

where D¯ is the mean diffusion coefficient, Dp is the diffusion coefficient for dislocations and Dva is the self-diffusion coefficient and f is the fraction of time that the diffusing atom spends within the dislocation. As the dislocation density increases, f increases, and since Dp > Dva , then D increases as well.

Nomenclature

187

Fig. 4.25. The effect of grain size on the character of diffusion in polycrystalline solids

This general formulation can also be applied to interface or surface diffusion occurring on external and internal surfaces of solids. In general, for defects in the lattice, the more loosely bound the atoms, the lower is the activation energy and the higher is the diffusion coefficient. So surface diffusion requires a lower activation energy than that for other forms of diffusion since each surface atom has only half the nearest neighbors as it does in the bulk, and generally: Qsurface < Qgb < Qp < Qva ,

and so

Dsurface > Dgb > Dp > Dva .

Nomenclature a A C Dyx Dgb D˜ Dlattice Dp Dtracer E f F G H J k n nm N pv P

Lattice constant Factor depending on geometry and diffusion mechanism Concentration Diffusion coefficient of species x via y Diffusion coefficient for grain boundary diffusion Interdiffusion coefficient Diffusion coefficient of lattice atom Diffusion coefficient for pipe diffusion Diffusion coefficient of tracer atom Energy Correlation (Haven) coefficient Helmholtz free energy Gibbs free energy Enthalpy Flux [cm−2 ] Boltzmann’s constant Number of defects Number of activated complexes Number of sites Probability that a lattice site is vacant Pressure

(4.75)

188

4 Point Defect Formation and Diffusion

Q R ra S T U ν¯ V z

α δ γ Γ Λ μ ν νE νr σ ω Ω

Activation energy Radius Radius of an atom Entropy Temperature internal energy Average velocity of atoms moving through barrier in activated complex, Eq. (4.50) Volume Number of nearest neighbors 1/6zA2 Width of the barrier in an activated complex Eq. (4.50); grain boundary width Stacking fault energy Jump frequency Jump distance Shear modulus Frequency; Poisson’s ratio Natural frequency of an oscillator Perturbed frequency of an oscillator Surface energy Jump frequency to a single site Volume of an atom

Subscripts a E f gb i,v m p r th

Atomic Natural component to ν Formation Grain boundary Interstitials, vacancies Migration Pipe Vibrational contribution to ν Thermal

Superscripts FP i,v mix

Frenkel pair Interstitials, vacancies Mixing

Acronyms SIA

Single interstitial atom

Problems

189

Problems 4.1 Many metals occur with both bcc and fcc structure, and it is observed that the transition from one structure to the other involves only insignificant volume change. Assuming no volume change, find the ratio Dfcc /Dbcc where Dfcc and Dbcc are the closest distances between metal atoms in the respective structures. 4.2 For a Ni lattice, calculate the following parameters for atomic chains along the (110) direction: a) the number of atoms per unit chain length b) the number of chains per unit area c) the product of the two. What is this product? 4.3 In the past, investigators have sometimes considered an interstitial atom as having been produced by the transfer of an atom from a normal lattice site to an interstitial site, thus resulting in a one-to-one correspondence between the concentrations of vacancies and interstitials. However, the equilibrium number of vacancies is generally orders of magnitude greater than the equilibrium number of interstitials at a given temperature. Explain. 4.4 The magnitude of the relaxation volume, |V | is greater than 1.0 for interstitials and is less than 1.0 for vacancies. Explain. 4.5 In terms of the jump frequency to a particular neighboring site, ω , and the lattice constant, a, what is the diffusion coefficient for impurity atoms whose equilibrium position is the octahedral interstitial site in: a) the fcc lattice b) the bcc lattice? 4.6 Consider a rigid crystal in the shape of a sphere of radius R. We create a small cavity of radius r (one atomic volume) in the center of the sphere. The material that was in this volume is spread uniformly over the surface of the sphere (assuming this can be done), increasing the radius of the sphere to R . a) Show that for an atomic radius of 0.15 nm and an intrinsic surface energy, σ ∼ 10 eV/nm2, the formation energy of a vacancy is of order 2 eV. b) If instead of a rigid solid, the crystal is treated as an elastic continuum, how would this affect the value of Efv you calculated for part (a)? Why? 4.7 Calculate the diffusivity of interstitials and vacancies in a piece of copper at 484 ◦C. Neglect the contributions of mixing entropy. Use 0.361 nm for the lattice constant. Also, calculate the diffusion coefficient for diffusion of atoms by vacancy self-diffusion. Why is this so much lower than the diffusivity of vacancies? Take γ = 1. 4.8 In a laboratory experiment conducted at 10 ◦C below the melting point of copper, 0.02% of the atom sites are vacant. At 500 ◦C, the vacant atom fraction was 5.7 ×10−8. a) What is the vacancy formation energy? b) How many vacancies are there per cm3 at 800 ◦C?

190

4 Point Defect Formation and Diffusion

References 1. Ullmaier H, Schilling W (1980) Radiation damage in metallic reactor materials. In: Physics of Modern Materials, vol. I. IAEA, Vienna 2. Hackett MJ, Was GS, Simonen EP (2005) J ASTM Int 2(7) 3. Thompson MW (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge 4. Shewmon PG (1989) Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA 5. Mrowec S (1980) Defects and Diffusion in Solids, an Introduction. Elsevier, New York 6. Smigelskas A, Kirkendall E (1947) Trans AIME 171:130 7. Darken L (1948) Trans AIME 175:184–201

5 Radiation-Enhanced Diffusion and Defect Reaction Rate Theory

We have developed an understanding of the formation of point defects, their motion or diffusion in a solid, and the configurations of some of the common types of defect clusters encountered in irradiated and unirradiated metals. Clearly, the formation, growth and dissolution of defect aggregates such as voids, dislocation loops, etc., depend upon the diffusion of point defects and their reaction with the defect aggregates. But they also depend upon the concentration of point defects in the solid. The concentration at any point and time is a balance between the production rate, and the loss rate of point defects and is adequately described by the point defect balance equations. The increase in diffusion or enhancement of atom mobility in an irradiated metal is due to two factors: (1) the enhanced concentration of the defects, and (2) the creation of new defect species. Recall that the diffusion of lattice atoms by way of the vacancy mechanism is given by: Dva = fv DvCv , where Dv is the vacancy diffusion coefficient, Cv is the vacancy concentration and fv is the correlation coefficient. Thus, increasing the concentration of vacancies will increase the diffusion coefficient for the atoms in the metal. However, if other mechanisms of diffusion are operative, such as interstitials or di-vacancies, then the total diffusion coefficient for atoms, Da is written as: Da = fv DvCv + fi DiCi + f2v D2vC2v + . . . and diffusion of atoms in the metal is increased by opening new channels via defect species which are usually not present in significant concentration at thermal equilibrium. Under irradiation, Da is also written as Drad . In this chapter, we will develop the transient and steady state solutions to the point defect balance equations in different temperature and microstructural regimes within the framework of radiation-enhanced diffusion [1, 2]. The solutions to the equations are used to determine the radiation-enhanced diffusion coefficient. Reaction rate theory is then presented to develop an understanding of how point defects interact with the various defect aggregates. Radiation-enhanced diffusion and defect reaction rate theory are essential to understanding the evolution of the irradiated microstructure developed in Chaps. 6–10.

192

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.1 Point Defect Balance Equations The development of radiation-induced vacancy and interstitial concentrations occurs due to competing processes. Frenkel defects are created from the collisions between high-energy particles and lattice atoms. These defects can be lost either through recombination of vacancies and interstitials or by reaction with a defect sink (void, dislocation, dislocation loop, grain boundary or precipitate). The local change in defect concentration of the various defect species can be written as the net result of (1) the local production rate, (2) reaction with other species, and (3) diffusion into or out of the local volume or the divergence of the flow. The main reactions we will focus on in this treatment are vacancy–interstitial recombination (v + i → , where represents a lattice site) and point defect reactions with sinks (v + s → s, and i + s → s). These competing processes can be mathematically described by the chemical rate equations: dCv = K0 − KivCiCv − KvsCvCs dt dCi = K0 − KivCiCv − KisCiCs , dt where Cv = vacancy concentration Ci = interstitial concentration K0 = defect production rate Kiv = vacancy–interstitial recombination rate coefficient Kvs = vacancy–sink reaction rate coefficient Kis = interstitial–sink reaction rate coefficient

(5.1)

The terms Kiv , Kvs , Kis are rate constants of the general form, K jX that describe the loss rate of point defects, j per unit point defect concentration to sinks of type, X. Similar equations can be written for defect agglomerates such as di- and trivacancies and interstitials. Note that the equations are non-linear differential equations and they are not mutually symmetric with respect to vacancy and interstitial concentrations because of the difference in Kis and Kvs , making an analytical solution difficult. The term “chemical” refers to homogeneous reactions, where the rate depends only on concentration (“law of mass action”) and not on the local distribution C(r) of the reactants. Thus, uniformity and thereby chemical kinetics require that ∇C ≈ 0. This gives rise to a problem when considering localized sinks, e.g., dislocations, grain boundaries, voids, precipitate interfaces, etc. Such local sinks violate the supposition of spatial uniformity in the host metal in that there is now locally, a directed net flow of mobile point defects toward the closest sinks. The divergence of the flow is equivalent to another “reaction” term, ∇ · D∇C in the kinetic balance equations. The locally valid rate equations are:

∂ Cv = K0 − KivCiCv − KvsCvCs + ∇ · Dv∇Cv ∂t ∂ Ci = K0 − KivCiCv − KisCiCs + ∇ · Di∇Ci . ∂t

(5.2)

5.1 Point Defect Balance Equations

193

The solution to these equations requires the statement of boundary conditions in addition to the initial local concentrations of the mobile defects (vacancies and interstitials). However, we can assume that ∇C ≈ 0 if the mean defect separation is greater than the mean distance between sinks, that is, the sink density is higher than the defect density. This amounts to treating the sink as being uniformly distributed and Eq. (5.1) applies. We consider the following model for the solution to Eq. (5.1). A pure metal is irradiated to produce only single vacancies and single interstitials in equal numbers with no spatial correlation of the interstitial with its vacancy. The interstitials and vacancies migrate by random walk diffusion, annihilating each other by mutual recombination or at unsaturable fixed sinks. Sinks and defects are distributed homogeneously in the metal. The diffusion coefficient of the metal is given by the sum of terms due to its diffusion by vacancies and interstitials. The model will have the following limitations: 1. The model applies to a pure metal. Binding of defects to atomic species and limitation of defect motion due to binding and correlation effects are neglected, f = 1. 2. The sink concentrations and strengths are time-independent, or unsaturable. 3. Other than mutual recombination, defect–defect interactions (e.g., the formation of di-vacancies or di-interstitials) are ignored. 4. Bias factors for diffusion of defects to sinks are set to unity (no preferential absorption of specific point defects at specific sinks). 5. Diffusion terms in and out of a specific volume are not considered. 6. The thermal equilibrium vacancy concentration is neglected. The rate constants are as follows: Kiv = 4π riv (Di + Dv) ≈ 4π riv Di

(5.3)

since Di Dv , Kis = 4π ris Di

(5.4)

Kvs = 4π rvs Dv ,

(5.5)

where riv , rvs and ris are interaction radii for the reaction between the species given by the subscripts and represent the radii of surfaces such that if crossed by the defect, it is annihilated. The terms Di and Dv are the interstitial and vacancy diffusion coefficients, respectively. The production term, K0 , is the effective point defect production rate in that it refers to the production of only freely migrating defects that can give rise to long-range diffusion (see Chap. 3). The derivations of the terms in Eqs. (5.3) and (5.4) will be given in the Sect. 5.3. Note that since the rate constants can differ by several orders of magnitude, the equations are stiff. That is, the time increment needed to follow interstitial motion is orders of magnitude too small to show any vacancy motion. Therefore, the equations must be solved using numerical techniques for stiff equations. But we can gain

194

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

insight into the processes by looking at analytical solutions to limiting cases. For example, the defect concentrations initially increase linearly with Cv = Ci = K0t. Further development depends on the values of the temperature and sink concentration, Cs . We will develop analytical solutions to Eq. (5.1) for four different regimes (combinations of T and Cs ); (1) low T and low Cs , (2) low T and intermediate Cs , (3) low T and high Cs , and (4) high T . 5.1.1 Case 1: Low Temperature, Low Sink Density The approximate solutions to Eq. (5.1) for low temperature and low sink density are given in Fig. 5.1. Initially, defect concentrations build up according to dC/dt = K0 with Ci ∼ Cv , so Ci = Cv = C = K0t. Initially, the concentrations are too low for either recombination or sinks to have an effect on the buildup. The buildup of point defects will start to level off when the production rate is compensated by the recombination rate. In the time regime where the production rate is balanced by the recombination rate, we drop the last two terms from Eq. (5.1) and solve for the “quasi-steady state” concentrations: dC = K0 − KivC2 = 0 (C = Ci = Cv ) , dt

(5.6)

Fig. 5.1. Log-log plot of vacancy and interstitial concentration vs. time for case (1) low temperature and low sink density (after [2])

5.1 Point Defect Balance Equations

with the solution: 1/2 K0 . C= Kiv Equating this concentration with that during the buildup phase: 1/2 K0 K0t = , Kiv

195

(5.7)

(5.8)

yields the time at which losses to recombination compensate for the production rate from irradiation: t = τ1 = (K0 Kiv )−1/2 ,

(5.9)

where τ1 is a time constant or characteristic time for the onset of mutual recombination. Eventually, the interstitials (first) and then the vacancies (later) will begin to find the sinks and sinks will start to contribute to annihilation. Ci and Cv remain approximately equal until a time τ2 , which is the time constant for the process of interstitials reacting with the sinks. Because Di > Dv , more interstitials are lost to sinks than vacancies, which is described by: dCi = −KisCiCs , dt

(5.10)

so the interstitial concentration will decay and the vacancy concentration will rise (since their only sink is interstitials and interstitials are being lost to sinks), yielding:

K0 KisCst 1/2 Cv (t) = Kiv (5.11)

1/2 K0 Ci (t) = . Kiv KisCst (The derivation of Eq. (5.11) is Problem 5.15 at the end of the chapter.) The time at which these equalities occur is obtained by equating the concentrations in the bounding time regimes of quasi-steady state and buildup of interstitials/decay of vacancies (Fig. 5.1): 1/2

K0 K0 KisCst 1/2 Cv = = Kiv Kiv (5.12) 1/2

1/2 K0 K0 Ci = = , Kiv Kiv KisCst and solving for the time yields the time constant for the onset of the buildup regime: t = τ2 = (KisCs )−1 .

(5.13)

196

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

After a while, at time τ3 , true steady state will be achieved. τ3 is the time constant for the slowest process, which is the interaction of vacancies with sinks. Solving Eq. (5.1) for the steady state concentration of vacancies and interstitials by setting dCv / dt = dCi / dt = 0 gives:

1/2 K 2 C2 K0 Kis KisCs + + is 2s 2Kiv Kiv Kvs 4Kiv

2 C2 1/2 KvsCs K0 Kvs Kvs s Ciss = − + + . 2Kiv Kiv Kis 4Kiv2

Cvss = −

(5.14)

Since vacancies and interstitials are produced in equal numbers and equal numbers are lost to recombination, the loss of each to sinks must be equal at steady state, and: KvsCv = KisCi .

(5.15)

For the case of low temperature and low sink density, Cs is small, and the vacancy and interstitial concentrations in Eq. (5.14) are approximated as: K0 Kis ∼ ∼ K0 Kvs . Cvss = ; Ciss = (5.16) Kiv Kvs Kiv Kis Equating these expressions to those from the previous (buildup) region gives:

Cv =

K0 KisCst Kiv

1/2 =

K0 Kis Kiv Kiv

1/2 .

(5.17)

and solving for the time gives the time constant for the onset of steady state: t = τ3 = (KvsCs )−1 .

(5.18)

The buildup shown in Fig. 5.1 is really a schematic and not the actual buildup. The transitions between regimes are not so sudden. For example, if the sink density is assumed to be zero, the exact solution to Eq. (5.1) is: "

K0 Cv (t) = tanh Kiv K0t . (5.19) Kiv 5.1.2 Case 2: Low Temperature, Intermediate Sink Density Increasing the sink density has the effect of bringing τ2 closer to τ1 (see Fig. 5.2). That is, the region of mutual recombination is shrunk at the expense of annihilation at sinks. In fact, when:

τ1 = τ2 or (K0 Kiv )−1/2 = (KisCs )−1 , the plateau disappears.

(5.20)

5.1 Point Defect Balance Equations

197

Fig. 5.2. Log-log plot of vacancy and interstitial concentration vs. time for case (2) low temperature and intermediate sink density (after [2])

5.1.3 Case 3: Low Temperature, High Sink Density The main effect of a high sink density is that interstitials find the sinks before they find vacancies because Cs Cv at short time (Fig. 5.3). That is, the time to reach linear buildup (loss of interstitials to sinks), τ2 , becomes shorter than the time to reach quasi-steady state due to vacancy–interstitial interaction, τ1 . In this case, the interstitial concentration comes into a quasi-steady state with production and annihilation at sinks: dCi = 0 = K0 − KisCiCs , (5.21) dt resulting in the quasi-steady state concentration: Ci =

K0 . KisCs

(5.22)

Equating interstitial concentrations in the linear buildup regime with the quasisteady state regime: K0t =

K0 , KisCs

(5.23)

and solving for t gives the value for the time constant τ2 : t = τ2 = (KisCs )−1 .

(5.24)

198

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.3. Log-log plot of vacancy and interstitial concentration vs. time for case (3) low temperature and high sink density (after [2])

Note that since interstitials have found the sinks before finding the slower vacancies, the vacancy concentration continues to rise according to Cv = K0 t. A competition soon arises between annihilation of interstitials at sinks and recombination with vacancies: KisCiCs = KivCiCv ∼ = KivCi K0t ,

(5.25)

yielding the time constant for the transition between the regimes where interstitials go to sinks and mutual recombination dominates: t = τ4 =

KisCs . Kiv K0

(5.26)

In the regime following τ4 , Cv rises but more slowly, and Ci decreases slowly according to: Cv = (K0 KisCs t/Kiv )1/2 Ci = (K0 /Kis KivCst)1/2 .

(5.27)

5.1 Point Defect Balance Equations

199

Steady state arrives at:

τ3 =

1 , KvsCs

(5.28)

with

1/2 Kis2 Cs2 KisCs K0 Kis =− + + 2Kiv Kiv Kvs 4Kiv2

2 C2 1/2 K0 Kvs Kvs KvsCs s Ciss = − + + . 2Kiv Kiv Kis 4Kiv2

Cvss

(5.29)

Note that the steady state concentrations are the same as Eq. (5.14) given earlier in case (1), but without the simplification of dropping the terms in Cs since in this case, the sink density is high and cannot be neglected. 5.1.4 Case 4: High Temperature At high temperature, the defect annihilation rate at the sinks keeps the concentration of interstitials low (Fig. 5.4). Since recombination does not contribute much, the rate equations become: dCv = K0 − KvsCsCv dt dCi = K0 − KisCsCi , dt

(5.30)

with steady state solutions: Cv =

K0 , KvsCs

Ci =

K0 , KisCs

(5.31)

with characteristic times given by: interstitial annihilation at sinks: vacancy annihilation at sinks:

K0 ⇒ t = τ2 = (KisCs )−1 (5.32) KisCs K0 K0t = ⇒ t = τ3 = (KvsCs )−1 . (5.33) KvsCs K0t =

The time evolution of vacancy and interstitial concentrations displayed in Fig. 5.4 ignores the presence of thermal vacancies, which may be significant at higher temperatures. The buildup of radiation-induced vacancies and interstitials at high temperature, including an initial presence of thermal equilibrium vacancies is shown in Fig. 5.5. Note the effect of sink (dislocation) density and defect production rate.

200

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.4. Log-log plot of vacancy and interstitial concentration vs. time for case (4) high temperature (after [2])

Fig. 5.5. Steady state (a) vacancy and (b) interstitial concentrations in an irradiated metal at a high production rate (solid line) and at a low defect production rate (dashed line). The upper and lower curves for each defect production rate represent small and large dislocation densities, respectively (after [3])

5.1 Point Defect Balance Equations

201

Table 5.1. Time constants for rate-limiting processes in the point defect balance equations Time constant

Value

Process

τ1 τ2 τ3

(K0 Kiv )−1/2 (KisCs )−1 (KvsCs )−1 K Cs τ12 /τ2 = is K0 Kiv

Onset of mutual recombination Onset of interstitial loss to sinks Onset of vacancy loss to sinks

τ4

Mutual recombination dominates interstitial loss to sinks

Figure 5.5a shows that increasing the sink density lowers the vacancy concentration since sinks absorb the vacancies (loss term is proportional to Kvs ). Also for a fixed sink density, a higher displacement rate results in a higher vacancy concentration because the production rate is higher than the loss rate to sinks. The same is true for interstitials shown in Fig. 5.5b. The kinks in the interstitial concentration curves correspond to the temperature at which vacancies become mobile and contribute to interstitial loss by mutual recombination as in Fig. 5.3. Comparing Figs. 5.5a,b shows that the equilibrium concentration of interstitials is negligible over the practical range of reactor component temperatures, while this is not the case for vacancies. The main objective of solving the point defect balance equations is to obtain values for Ci and Cv to determine Drad , which is just the sum of Ci Di and Cv Dv . The preceding discussion shows that we can interpret radiation-enhanced diffusion experiments after an isothermal irradiation at a constant flux for a time t in terms of characteristic times. Table 5.1 summarizes the time constants for the various ratelimiting mechanisms. For low sink density, recombination dominates at short times, followed by interstitial annihilation at sinks and then vacancy annihilation at sinks, which is the slowest process and controls the achievement of steady state. At high sink density, interstitial annihilation at sinks dominates early, followed by mutual recombination and then vacancy loss to sinks. As a rule, when τ1 < τ2 , mutual recombination dominates and when τ2 < τ1 , sinks dominate. In summary, the key factors affecting Ci and Cv are production rate, defect mobility and sink concentration. 5.1.5 Properties of the Point Defect Balance Equations The point defect balance equations and their solutions possess interesting properties, which provide further insight into the behavior of vacancies and interstitials in the diffusion of lattice atoms. They are the following: 1. The vacancy concentration referred to in the last section is really Cv −Cv0 where Cv0 is the thermal equilibrium concentration of vacancies. In high-temperature irradiations (T /Tm ≥ 0.5), this concentration is non-negligible. However, over all irradiation temperatures of interest, Ci0 /Ci 1.

202

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

2. In the absence of sinks and thermal vacancies, Cv can be exchanged with Ci , that is, Cv = Ci at any instant: dCv = K0 − KivCiCv dt dCi = K0 − KivCiCv . dt

(5.34)

Since Drad = DiCi + DvCv , and Ci = Cv , but since Di Dv , then interstitials contribute much more to atom mobility than do vacancies. 3. If there is only one type of sink, then at steady state: K0 = KivCiCv + KvsCvCs K0 = KivCiCv + KisCiCs ,

(5.35)

KvsCv = KisCi ,

(5.36)

or

and the absorption rate of interstitials and vacancies at sinks is equal, or the net absorption rate at the sink is zero. Even for the case of multiple sink types, if the sinks have the same “strength” for vacancies and interstitials, then the net flow to any sink is zero. 4. Inclusion of sink terms violates the symmetry with respect to Ci and Cv because of the different values of K (Kvs = Kis ). Symmetry is present in the steady state with regard to DiCi and DvCv (since Kis α Di and Kvs α Dv ). The physical consequence is that vacancies and interstitials contribute to atom mobility to the same extent and their actions cannot be discriminated. At steady state: 0 = K0 − KivCiCv − Kvs DvCvCs 0 = K0 − KivCiCv + Kis DiCiCs ,

(5.37)

where the K terms have been written as K = K D, giving: DvCv Kvs Cs = DiCi Kis Cs .

(5.38)

∼ K , then D C = D C which means that vacancies and interstitials So if Kvs v v i i is contribute equally to atom mobility. Even though the steady state concentration of interstitials is much lower than the steady state concentration of vacancies, they each contribute equally to atom mobility because of the faster rate of diffusion of interstitials. For any particular sink to grow, it must have a net bias for either vacancies or interstitials. In real metals, Kvs and Kis are not equal. Specific sinks have a bias for certain point defects, allowing that sink to grow. This behavior is described in more detail Sect. 5.3.

5.2 Radiation-Enhanced Diffusion

203

5.1.6 Deficiencies of the Simple Point Defect Balance Model The simple point defect model neglects numerous features of realistic systems that must be incorporated in order to obtain accurate results. For example, no account is taken for changing sink strengths, which occur as dose buildup continues due to the formation of depleted zones and defect clusters. Also, sink bias is neglected. Bias is an important factor affecting the development of the irradiated microstructure as will become evident in Chaps. 7 and 8. Defect–defect interaction and defect– impurity interaction have also been neglected. Defect–defect interaction will be important in the formation of void and interstitial loop nuclei and cannot be neglected if larger clusters are to be properly accounted for. These small clusters will serve as traps or sinks for mobile defects. In fact, vacancy clusters have been found to increase Drad in the mutual-recombination range, but are insignificant for high sink concentrations and temperatures where annealing to fixed sinks dominates [4]. Finally, the equations are unable to account for defect gradients (and in the simple form, for concentration gradients). These become very important in processes such as radiation-induced segregation (Chap. 6), in which defect fluxes give rise to concentration gradients in the alloying elements. Such processes may significantly alter the behavior of sinks and the bias of the sinks.

5.2 Radiation-Enhanced Diffusion In a pure metal, the diffusion coefficient under radiation is given by: Drad = DvCv + DiCi .

(5.39)

Because the concentrations of vacancies and interstitials under irradiation are much greater than those produced thermally, the radiation-enhanced diffusion coefficients are much larger than thermal diffusion coefficients. Despite the shortcomings, it is interesting to see how well the simple point defect balance equations are able to estimate the effect of irradiation on diffusion. Figure 5.6 is a plot of log Drad vs. logt for the case of annealed Ag-30% Zn at 40 ◦C irradiated with 2.5 MeV electrons at a flux of 3.7 ×1015 m−2 s−1 [2]. The thin solid lines are the interstitial and vacancy concentrations and the thick solid line is the their sum as calculated from Eq. (5.35) by Sizeman [2] and the dashed line is the experimental data. The experiment actually measures the Zener relaxation time, τz (see [1]), which is proportional to Drad . The experimental result confirms the existence of a maximum in Drad as in case (1) for low temperature and low sink density. This result also shows that the interstitial component dominates at times less than that to achieve steady state, τ3 , since Di > Dv (by assumption) and Ci > Cv for τ < τ3 . Another excellent example of calculation of Drad vs. measurement is provided by Rothman [5.1] for self-diffusion in copper at 200 ◦C in a crystal containing a dislocation density of 1011 m−2 under irradiation with a net damage rate,

204

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.6. Time dependence of Drad vs. lnt for both calculation (solid line) and measurement (dashed line). Thin solid lines are for the vacancy and interstitial components and the heavy solid line is the sum of the components (after [2])

K0 = 10−6 dpa/s (similar to that experienced by a fast reactor core structural material). In this case, Drad ∼ 6.5 ×10−21 m2 s−1 . Given that the thermal diffusion coefficient is ∼ 1.4 ×10−27 m2 s−1 , this represents an extremely large (> 106 ) increase due to irradiation. Figure 5.7 shows that at temperatures below 575 ◦C, Drad exceeds the thermal equilibrium self-diffusion coefficient for this defect production rate (curve 1). The various curves in Fig. 5.7 represent different combinations of production rates and defect densities. Note that at low temperature, mutual recomv /2 (all curves). At low bination dominates and Drad has an activation energy of Em 11 −2 sink density (10 dislocations m (curve 1), where ρd ∼ 4π rvsCs = 4π risCs ) the mutual recombination region ties indirectly to diffusion by thermal equilibrium vacancies with increasing temperature. At high sink densities, (1014 m−2 (curve 2) and 1015 m−2 (curve 3)), mutual recombination gives way to annealing at fixed sinks at a critical temperature, determined as follows. According to Eq. (5.36), for a single sink type: Ci Kis = Cv Kvs

or Ci =

Cv Kvs . Kis

(5.40)

5.2 Radiation-Enhanced Diffusion

205

Fig. 5.7. Calculated Drad for self-diffusion of copper as a function of temperature for different combinations of defect production rates and dislocation densities. 1: K0 = 10−6 dpa/s, ρd = 1011 m−2 , 2: K0 = 10−6 dpa/s, ρd = 1014 m−2 , 3: K0 = 10−6 dpa/s, ρd = 1015 m−2 , 4: K0 = 10−4 dpa/s, ρd = 1011 m−2 (after [1])

At steady state, Eq. (5.29) apply and they can be re-written in the following form: KisCs 4K0 Kiv 1/2 Cv = −1 1+ 2Kiv Kis KvsCs2 (5.41) KvsCs 4K0 Kiv 1/2 Ci = −1 . 1+ 2Kiv Kis KvsCs2 We define a parameter, η , such that:

η=

4K0 Kiv . Kvs KivCs2

(5.42)

Then using Eq. (5.41) Cv can be written as: Cv =

F(η )K0 , or Cv KvsCs = F(η )K0 . KvsCs

(5.43)

where: F(η ) =

2 [(1 + η )1/2 − 1] . η

(5.44)

Equation (5.43) shows that F(η ) determines the number of defects absorbed by sinks in relation to the total rate of formation of the defects. If η → 0, then

206

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

F(η ) → 1, i.e., all of the defects are lost to sinks and none to recombination. In the limit of large η , F(η ) ∼ 2/η 1/2 and F(η ) → 0, indicating that mutual recombination dominates defect loss. When F(η ) = 1/2, the loss of defects to sinks and recombination is equal. This occurs at a value of η of:

η =8=

4K0 Kiv . Kvs KisCs2

(5.45)

Equation (5.45) can be solved for the critical temperature below which mutual recombination will dominate, and above which loss to sinks will dominate. (The term η will be revisited in Chap. 8 in describing the effect of recombination on void growth). Using Eqs. (5.3), (5.4), and (5.5) for Kiv , Kis and Kvs , and defining = 4π r , gives: Kiv = 4π riv , Kis = 4π rvs and Kvs iv i −Em 4K0 Kiv Di0 exp kT 8= , (5.46) v i −Em Di exp −Em C2 Dv exp Kvs K s 0 is 0 kT kT v is the migration energy and Di,v is the pre-exponential factor in the difwhere Ei,m 0 fusion coefficient for interstitials and vacancies, respectively. Equation (5.46) simplifies to:

Tc =

k ln

v Em v 2D0Cs2 Kis Kvs K0 Kiv

.

(5.47)

At the highest temperatures, Drad is overwhelmed by thermal vacancies (all curves in Fig. 5.7), and increasing K0 to 10−4 dpa/s (curve 4) raises Drad in the mutual recombination range by a factor of 10. Figure 5.8 shows the radiation-enhanced diffusion coefficient calculated for a sample of nickel undergoing irradiation at a rate of 10−6 dpa/s for different sink annihilation probabilities, p, where p−1 is the average number of jumps of a defect between creation and annihilation at a sink [5]. The diffusion coefficient describing radiation-enhanced diffusion, Drad , is shown by the solid line. The dashed line to the left is the thermal diffusion coefficient and the solid horizontal line at the right is the diffusion coefficient due to ballistic mixing, Dm [6], and will be discussed in Chap. 10. The difference between the curves for Drad and Dth is the effect of radiation-enhanced diffusion. As shown, irradiation can result in a several orders of magnitude increase in the diffusion coefficient.

5.3 Defect Reactions Each of the terms in the point defect balance equation represents a reaction. The rate at which the reaction occurs will depend on the nature of the reacting species.

5.3 Defect Reactions

207

Fig. 5.8. Diffusion coefficient as a function of 1/T for a nickel-base alloy during irradiation at a displacement rate of 10−6 dpa/s. Drad is calculated from rate theory for various sink annihilation probabilities, p. The diffusion coefficient from displacement mixing is Dm and the thermal diffusion coefficient is Dth (from [5])

Following [3], we will develop expressions for the rates of each of the reactions in the point defect balance equation, as they will be used in describing processes such as void growth, dislocation climb, etc. We have seen that the motion of mobile point defects can be considered a random walk process. When one of these defects encounters a specie in the crystal to which it becomes tightly bound, one or both of the partners in the encounter is considered to disappear from the solid. Examples include a vacancy or interstitial intersecting a free surface, grain boundary, dislocation, void, etc., or a vacancy encountering a vacancy, an interstitial encountering an interstitial, or a vacancy encountering an interstitial. Clearly the rate of such reactions is proportional to the concentrations of both species, or: reaction rate of A and B = KABCACB reactions/cm3 s ,

(5.48)

where CA and CB are the concentration of species A and B in units of particles/cm3, and KAB is the rate constant of the reaction in cm3 /s. Reactions can be between two mobile particles (vacancy and interstitial at high temperature) or between one mobile and one stationary defect, e.g., low temperature where vacancies are immobile and interstitials are mobile, or between interstitials and dislocation, grain boundaries, voids, etc. There are two types of processes that will be of interest in dealing with the reaction between point defects and sinks. They are reaction rate-controlled and diffusion-controlled processes. In reaction rate-governed processes, there must be no macroscopic concentration gradients of either partner. If one partner is large compared to the atomic sized reactant, or if one is a strong sink, a concentration gradient may be established in the vicinity of the stationary defect. Reactions between point defects are examples of reaction rate-controlled processes. If a defect

208

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory Fig. 5.9. Locations of nearest neighbors for the formation of a di-vacancy in the fcc lattice (after [3])

concentration gradient is established, the overall process is governed by the rate of diffusion of the mobile species to the stationary sink. This is the case with free surfaces, voids and grain boundaries. These defects are usually not treated by reaction rate theory. As a first example of a reaction rate-controlled process, let us look at the vacancy–vacancy reaction. Consider the reaction: v + v → v2 ,

(5.49)

that proceeds in the forward direction only and is characterized by the rate constant K2v . In this example, one vacancy is assumed to be stationary and the other is mobile. The rate of di-vacancy formation per cm3 is: R2v = P2vCv

(5.50)

where Cv is the concentration of monovacancies and P2v is the probability per second that another vacancy jumps into a site that is a nearest neighbor to a particular vacancy (Fig. 5.9). A di-vacancy will form if a nearest neighbor site to a vacancy is occupied by another vacancy, thus P2v depends on the crystal structure. Taking the fcc lattice, all 12 nearest neighbor sites are equivalent, yielding: P2v = 12Px ,

(5.51)

where Px is the probability per second that another vacancy jumps into one of the nearest neighbor positions surrounding the vacancy. Px is proportional to: 1. The number of sites surrounding the nearest neighbor site from which another vacancy could jump (seven sites as shown by the dashed atoms in Fig. 5.9)

5.3 Defect Reactions

209

2. The probability that one of these lattice positions is occupied by a vacancy, Nv 3. The jump frequency of a vacancy, ω , or Px = 7Nv ωv ,

(5.52)

and we can write the vacancy site fraction as Nv = Cv Ω , where Cv is the volumetric vacancy concentration and Ω is the atomic volume. Back substitution of Eqs. (5.51) and (5.52) into Eq. (5.50) yields: R2v = 84ωΩ Cv2 [cm−3 s−1 ] .

(5.53)

Comparison with the definition of the reaction rate, Eq. (5.48) gives the reaction rate constant K2v : K2v = 84ωΩ .

(5.54)

In the fcc lattice, Dv = a2 ω , then K2v =

84Ω Dv . a2

(5.55)

Although the expression for the rate constant was derived for a vacancy–vacancy reaction, the same formulation applies to any reaction between any specie (e.g., impurity) that occupies substitutional positions in the fcc lattice. It can also be used for other lattice types, but the factor, 84, called the combinatorial factor is dependent on the crystal structure. The combinatorial factor is the solid state analog of the cross section in particle interactions. In the previous example, we forced one of the reactants to be stationary. When the reaction is between two mobile species, the rate is (KAB + KBA )CACB , where KAB is the rate constant calculated assuming that B is immobile and vice versa for KBA . Therefore, if both vacancies are mobile, the result would be multiplied by a factor of 2; K2v + K2v = 2K2v . Given this background, we now turn our attention to the various terms in the point defect balance equations in order to develop expressions for the reaction rate coefficients. 5.3.1 Defect Production The first term in the defect balance equations of Eq. (5.1) is the production rate of vacancies and interstitials and this was determined in Chap. 2, Eq. (2.125), where the term in brackets is given the designation, FP : K0 = ξ νFP σs N φ [cm−3 s−1 ] .

(5.56)

For stainless steel, νFP ∼ 30 Frenkel pairs per collision, σs ∼ 3 ×10−24 cm2 and N ∼ 7 ×1022 cm−3 . The term, ξ , is the displacement efficiency (Chap. 3) that accounts for the reduction in freely migrating point defects due to in-cascade recombination and clustering.

210

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.3.2 Recombination The second term in Eq. (5.1), KivCvCi is the recombination rate. The rate constant Kiv is the same for both vacancies and interstitials since they must recombine with each other at the same rate. Reactions between vacancies and interstitials are of great importance since the result is mutual annihilation or return to the perfect lattice. Assuming a stationary vacancy and a mobile interstitial, and that recombination only occurs when the interstitial jumps into a site that is nearest neighbor to the vacancy, we can determine the recombination rate constant for an octahedral interstitial in the fcc lattice. There are six octahedral sites as nearest neighbors to the vacant lattice site and each lattice site has eight octahedral nearest neighbors, giving a value of 48 for the combinatorial factor: Kiv =

48Ω Di . a2

(5.57)

However, this is a bit unrealistic since (1) the stable form of the interstitial is the split interstitial, and (2) the vacancy and interstitial are attracted to each other by virtue of their strain fields, causing spontaneous recombination to occur over distances greater than the nearest neighbor spacing. Therefore, a more realistic estimate of the combinatorial factor, ziv is ∼ 500: Kiv =

ziv Ω Di , and ziv ∼ 500 . a2

(5.58)

5.3.3 Loss to Sinks The loss term represents all the possible sinks for vacancy and interstitial loss. These sinks can be divided into three categories: 1. Neutral (unbiased) sinks show no preference for capturing one type of defect over the other type. The rate of absorption is proportional to the product of the diffusion coefficient of the point defect and the difference in the concentrations of the point defect in the bulk metal and at the sink surface. The types of sinks in this category are voids, incoherent precipitates and grain boundaries. 2. Biased sinks exhibit preferential attraction for one defect type over the other. Dislocations exhibit a stronger preference for interstitials than for vacancies. The bias is due to the drift of interstitials down the stress gradient near the dislocation core. Since absorption of interstitials enhances dislocation climb, the dislocation is an unsaturable sink. Two types of dislocations are considered; networks in unirradiated metal and from unfaulted Frank loops, and interstitial dislocation loops. 3. Variable bias sinks such as coherent precipitates act as traps, which capture a defect but preserve its identity until it is annihilated by the opposite type defect. Impurity atoms and coherent precipitates act as recombination centers with a limited capacity.

5.4 Reaction Rate-Controlled Processes

211

5.3.4 Sink Strengths Reaction rate constants describe the reaction and are designated a point defect and a sink (which may be another point defect), and are designated K jX where j is the mobile point defect and X is the sink. As such, they include the diffusion coefficient of the point defect as well as a description of the tendency for the reaction to occur. It is often useful to describe the tendency of a sink to absorb defects that is independent of the defect properties. The sink strength, with units of cm−2 , is such a description and it reflects the strength or affinity of a sink for defects. Sink strength is independent of defect properties for neutral sinks. The sink strength is defined as: absorption rate = K jX C jCX = k2jX C j D j ,

(5.59)

so K jX CX , Dj

k2jX =

(5.60)

or k2j = ∑ k2jX .

(5.61)

X

Both the rate constant and the sink strength are terms commonly used to describe the action of sinks on the defects in the solid. Physically, k−1 j is the mean distance a free defect of type j travels in the solid before becoming trapped. Before we treat the various sink types, we will first look at the rate constants for the two basic reaction processes; reaction rate-controlled processes and diffusionlimited processes. We begin with reaction rate-controlled processes.

5.4 Reaction Rate-Controlled Processes 5.4.1 Defect–Void Interaction For reactions where capture is controlled by the rate at which the point defects enter the trap site, we can use Eq. (5.58). For defect–void reactions, the term to be determined is the combinatorial factor. For a void, the number of lattice points on the surface of the sphere is 4π R2/a2 , where the area occupied by a lattice point is approximated at a2 . The rate constant then becomes: KvV =

4 π R 2 Ω Dv 4 π R 2 Dv , = a4 a

2 where Ω ∼ a3 , kV =

where ρV is the concentration of voids in the solid.

4 π R2 ρ V , a

(5.62)

212

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.4.2 Defect–Dislocation Interaction Consider a cylinder about a dislocation line whose axis is coincident with the dislocation line such that capture is certain for any vacancy entering the cylinder (Fig. 5.10). The cylinder consists of zvd atomic sites on each of the crystal planes intersected by the dislocation line. The cylinder defines the capture radius of the dislocation, or the radius inside which entering defects are lost to the sink. If the spacing between atom planes in the lattice is ∼ a, then there are zvd /a capture sites per unit length of dislocation. Letting ρd be the density of dislocation lines in the crystal (in units of centimeters of dislocation line per cm3 of solid or cm−2 ), then there are zvd ρd /a capture sites per unit volume. If the concentration of vacancies per unit volume is Cv , then the vacancy site fraction is Cv Ω . For a vacancy jump rate of ω , the rate of vacancy capture rate by the dislocation per cm3 is: Rvd =

zvd ρd Cv Ω ω [cm−3 s−1 ] . a

(5.63)

Since Ω ∼ a3 and Dv = a2 ω , we have: 2 = zvd ρd Rvd = Dv zvd ρdCv and reaction rate constant Kvd = Dv zvd , kvd 2 Rid = Di zid ρdCi and reaction rate constant Kid = Di zid , kid = zid ρd

(5.64)

and zvd = zid .

5.5 Diffusion-Limited Reactions Reactions between defects and sinks cannot always be characterized as reaction ratelimited. Reactions driven by defect concentration gradients are diffusion-limited and must be treated differently. Such reactions are defect–void, defect–grain boundary and sometimes defect–dislocation interactions. Following [3], these reactions are addressed here starting with defect–void reactions.

Fig. 5.10. Capture volume around a dislocation line, defined by the cylinder of radius Rd and with sink sites lying on crystal planes separated by a distance a

5.5 Diffusion-Limited Reactions

213

5.5.1 Defect–Void Reactions Consider the case of ρV voids per unit volume, each of radius, R, which absorb a particular type of point defect present in the solid and between the spherical sinks. Focusing on a single sphere, the unit cell or capture volume surrounding each sphere is defined as the portion of the solid that can be associated with each sphere. The radius of the capture volume (see Fig. 5.11) around each sphere is defined by: 4 π R3 ρV = 1 . (5.65) 3 The diffusion equation for the point defects will be solved in the spherical shell R ≤ r ≤ R. The concentration of point defects at a radial position r in the capture volume at time t is denoted by C(r,t). The definition of the capture volume implies that there is no net flux of point defects across the boundary at r = R which is written as: ∂C =0, (5.66) ∂r R and the point defect concentration at the surface of the sphere is: C(R,t) = CR .

(5.67)

The value of CR depends on the process. For insoluble gas atoms where the spheres represent gas bubbles, CR = 0. For bubbles or voids where the point defects are 0 , the thermal equilibrium defect concentration. vacancies or interstitials, CR = Cv,i If the defects are created uniformly in the capture volume and no sinks other than the sphere are present, then the concentration C(r,t) is determined by solution of the volumetric diffusion equation with a volumetric source term: D ∂ ∂C ∂C = 2 (5.68) r2 + K0 , ∂t r ∂r dr where D is the diffusion coefficient of the defects (assumed to be independent of concentration) and K0 is the defect production rate per unit volume given by Eq. (5.56).

Fig. 5.11. The unit cell for determination of the diffusion-controlled rate constant for defect absorption by a spherical sink

214

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

When a solid is irradiated at a temperature where point defects are mobile, the loss of particles to the sink is partially compensated by the production rate so the ∂C ∼ 0 and Eq. (5.61) can be approxiconcentration changes slowly with time ∂t mated as: D d 2 dC (5.69) r = −K0 . r2 dr dr The solution to Eq. (5.69) subject to the boundary conditions given by Eqs. (5.66) and (5.67) is:

K0 2R2 (r − R) 2 C(r) = CR + − r − R2 . (5.70) 6D rR Since in many cases, the capture volume radius is much larger than the sink radius and the defect concentration changes rapidly only very close to the sink, the capture volume is divided into two regions (Fig. 5.12). In region 1 the diffusion term is much greater than the source term and Eq. (5.69) can be approximated by: 1 d 2 dC r =0, (5.71) r2 dr dr with boundary conditions: C(R) = CR

(5.72)

C(∞) = C(R) .

(5.73)

The solution of Eq. (5.71) subject to the boundary conditions given by Eqs. (5.72) and (5.73) gives:

R C(r) = CR + [C(R) − CR ] 1 − . (5.74) r The flux of particles at the void surface is defined by: dC . J = −D dr R

(5.75)

Using Eq. (5.70) gives: J=

−D[C(R) − CR ] . R

(5.76)

The absorption rate of point defects by the void is: −(4π R2)J = 4π RD[C(R) − CR] .

(5.77)

Requiring that point defects produced in the capture volume be absorbed by the void gives: 4 π (R3 − R3)K0 = 4π RD[C(R) − CR ] . 3

(5.78)

5.5 Diffusion-Limited Reactions

215

Fig. 5.12. Regions of interest in the solution of the diffusion equation in a spherical shell with a uniform volumetric production rate of defects

If R3 R3 , the balance becomes: C(R) = CR +

K0 R3 . 3RD

(5.79)

Assuming that C(R) CR in Eq. (5.56) and replacing C(R) by C, we obtain the total rate of diffusion-controlled absorption of point defects by the void by multiplying Eq. (5.77) by the number of voids per unit volume ρV : Rate of absorption/cm3 = 4π RDρVC .

(5.80)

The rate constant for diffusion-controlled reaction of point defects and a perfect spherical sink of radius R is then: KiV = 4π RDi , KvV = 4π RDv , 2 = 4 π Rρ V , kV

(5.81)

where the subscripts of K refer to the reacting species, vacancies or interstitials (v, i) and voids, V . 5.5.2 Defect–Dislocation Reactions Diffusion-controlled reactions between defects and dislocations occur in much the same way as in the case of spherical sinks, but in cylindrical coordinates. Taking the capture radius of the sink to be Rd and the dislocation density to be ρd , we define the unit cell such that: (π R2 )ρd = 1 . The diffusion equation is: D d dC r + K0 = 1 r dr dr

(5.82)

(5.83)

216

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

with boundary conditions:

C(Rd ) = CRd dC =0, dr R

(5.84) (5.85)

and solution: C(r) = CRd +

2

r − R2d K0 R2 r − 1/2 . ln 2D Rd R2

(5.86)

Analogous to the case for spherical sinks, in region 1, but in cylindrical geometry instead, the diffusion equation is: dC 1 d r =0, (5.87) r dr dr with boundary conditions: C(Rd ) = CRd C(R) = C ,

(5.88) (5.89)

with solution: C(r) = CRd + [C(R) − CRd ]

ln(r/Rd ) . ln(R/Rd )

The flux of defects to the dislocation line is: −D[C(R) − CRd ] dC . = J = −D dr Rd Rd ln(R/Rd )

(5.90)

(5.91)

The absorption rate per unit length of dislocation line = −(2π Rd)J =

2π D[C(R) − CRd ] . ln(R/Rd )

(5.92)

The rate of defect production in the capture volume = π (R2 − R2d )K0 ,

(5.93)

and since all defects produced in the capture volume are captured by the dislocation: 2π D[C(R) − CRd ] = π (R2 − R2d)K0 , ln(R/Rd )

(5.94)

and C(R) = CRd +

K0 R2 ln(R/Rd ) for Rd /R 1 , 2D

(5.95)

5.6 Mixed Rate Control

217

so from Eq. (5.91) the rate of defect capture by dislocations per unit volume = 2π DρdC , and the rate constants for vacancies and interstitials are: ln(R/Rd ) 2 π Dv ln(R/Rvd ) 2 π Di , Kid = ln(R/Rid )

(5.96)

2πρd ln(R/Rvd ) 2πρd 2 . = kid ln(R/Rid )

(5.97)

Kvd =

and 2 kvd =

Note that the combinatorial factors for vacancies and interstitials differ by the capture radius. The capture radius for interstitials is slightly greater than that for vacancies and is the origin of the dislocation bias for interstitials.

5.6 Mixed Rate Control Mixed rate control occurs when the reaction rate is determined by a combination of processes. We can determine the rate constant for the combined processes by adding the reciprocals of the rate constants to give the resistance due to series steps of diffusion and surface attachment. For the case of voids, we use the rate constants given by Eqs. (5.62) and (5.81), and: 1 1 1 = + , Keff Kreaction Kdiffusion

(5.98)

to yield the effective rate constant: Keff =

4π RD a , 1+ R

2 = keff

4 π Rρ V a . 1+ R

(5.99)

For large spheres, a/R → 0 and the rate constant is that for diffusion only. This result shows that reaction rate limitations to capture kinetics for spherical sinks are only significant if the sphere radius is small, approaching the lattice constant. For dislocations, the capture rates calculated from a diffusion-controlled process vs. a reaction rate-controlled process are: 2π D ln(R/Rd ) Kreaction = zd D ,

Kdiffusion =

(5.100)

218

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

giving the effective rate constant for mixed-control: Keff =

D , 1 ln(R/Rd ) + zd 2π

2 keff =

ρd . 1 ln(R/Rd ) + zd 2π

(5.101)

Consider zd to be the area of a circular region of radius Rd divided by the number of atoms per unit area. For the (100) plane of the fcc lattice, the number of atoms/unit area is 2/a2 a/cm2 and: Kreaction /D = zd /D =

2π R2d = 24 for Rd ∼ 0.6 nm and a ∼ 0.3 nm . a2

For a dislocation line density of 1010 cm−2 , Kdiffusion /D = ture of defects by dislocations is diffusion-controlled.

(5.102)

2π = 1.4. So capln(R/Rd )

5.7 Defect–Grain Boundary Reactions Interactions between point defects and grain boundaries are important in the case of radiation-induced segregation, discussed in Chap. 6. Following the analysis of Heald and Harbottle [7], the sink strength of the grain boundary is determined by considering a spherical grain of radius a, with grain boundary defect concentration equal to the thermal equilibrium value, which will be neglected compared to the irradiated-induced concentration. The loss to sinks within the grain is: k2 DC = (zd ρd + 4π RVρV )DC ,

(5.103)

where k2 is the sink strength for the grain interior due to dislocations and voids, and the diffusion equation is: d2C 2 dC K0 + − k 2C = 0 , + dr2 r dr D

(5.104)

subject to boundary conditions C(r = a) = 0 and C(r = 0) = finite. The solution to Eq. (5.104) subject to the boundary conditions is:

K0 a sinh(kr) C(r) = 1− , (5.105) Dk2 r sinh(ka) and the total flow of point defects to the grain boundary, A is: 4π K0 a ∂ C = [ka cot(ka) − 1] . A = −4π r2D ∂ r r=a k2

(5.106)

5.8 Coherent Precipitates and Solutes

219

Written in rate theory formalism, Eq. (5.106) becomes: A = zgb DC0 ,

(5.107)

where zgb is the sink strength for an individual grain boundary and C0 is the concentration at the grain center (r = 0):

ka K0 1− C0 = C(r = 0) = . (5.108) Dk2 sinh(ka) From Eqs. (5.106), (5.107), and (5.108), the grain boundary sink strength, zgb is

ka cosh(ka) − sinh(ka) zgb = 4π a . (5.109) sinh(ka) − ka For small grains and low sink strengths, ka → 0, and: zgb (ka → 0) = 8π a = 4π d ,

(5.110)

where d(= 2a) is the grain diameter. When sink strength is large, ka → ∞, and: zgb (ka → ∞) = 4π ka2 = π kd 2 .

(5.111)

The grain boundary sink strength is the product of zgb and the grain density in grains per unit volume, or ρgb = 6/π d 3, giving: 2 kgb (ka → 0) = 24/d 2 ,

K jgb = 4π D j d ,

(5.112)

2 (ka → ∞) = 6k/d , kgb

K jgb = π kD j d 2 ,

(5.113)

and

where j = i or v. Generally, k2 ∼ 1011 cm−2 and d > 10−3 cm so that Eq. (5.113) is the appropriate expression for the grain boundary sink strength. In fact, the grain boundary sink strength is given by Eq. (5.113) whenever (zd ρd + 4π RVρV ) > 1/d.

5.8 Coherent Precipitates and Solutes These types of sinks are known as variable bias sinks in that they act as traps for vacancies and interstitials rather than as infinite sinks in which the defect loses its identity after being absorbed. The source of the attraction of vacancies and interstitials to the trap is the relief of the strain field produced by the coherency between the trap and the lattice. The coherent precipitate is of a structure in which the lattice planes of the precipitate are continuous with those of the matrix, but due to the difference in lattice parameters, there is a strain field at the interface where the lattice planes from each are forced to match. The over- or undersized solute is a limiting

220

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory Fig. 5.13. Diffusion-controlled reaction between vacancies and a grain boundary

case of a coherent precipitate. The trap strength is limited by the capacity of the interface to hold or trap a defect until the anti-defect arrives and results in annihilation. Hence, no matter accumulates at this defect and thermal emission does not occur. The interface does exhibit a bias for defects and this bias is a function of the biased sinks in the solid. For example, if the biased sinks in the solid favor interstitials, then ki2 > kv2 and the trap interface will acquire slightly more vacancies than interstitials. This excess of vacancies then causes the trap surface to become a more effective sink for interstitials than for vacancies. The biases for the trap are denoted by Yv and Yi (Brailsford and Bullough [8] and Olander [3] provide detailed analyses of the bias factors), and the absorption rates of vacancies and interstitials at the trap is given by: ACP v = 4π RCPDvCv ρCPYv = KvCPCv ρCP ACP i = 4π RCPDiCi ρCPYi = KiCPCi ρCP .

(5.114)

If there can be no steady state accumulation of defects at the trap, then there is no net matter flow to or from the sinks and: 4π RCP ρCPCvYv = 4π RCP ρCPCiYi ,

(5.115)

so Yi =

DvCv Yv , DiCi

(5.116)

and the rate constants and sink strengths are: KvCP = 4π RCP DvYv ;

2 kvCP = 4π RCP ρCPYv

KiCP = 4π RCP DiYi ;

2 kiCP = 4π RCPρCPYi .

(5.117)

So variable bias sinks play an interesting role in that they adjust their preference for point defects in response to the relative sink strengths in the bulk. The reaction rate constants for the various reactions are summarized in Table 5.2 for the various defect–defect, and defect–sink reactions.

v,i + coherent ppt

Diffusion control

v,i + grain boundary

Mixed rate control

Reaction rate control

Diffusion control

v,i + dislocation

Mixed rate control

Diffusion control

Reaction rate control

v,i + void

v+i

i+i

v+v

Reaction

Di = ln(R/Rid ) 1 + zid 2π

KiCP = 4π RCP DiYi

2 kigb = Di d 4 3 Kigb = 6kDi d 5

KvCP = 4π RCP DvYv ,

2 kvgb = Dv d 4 3 Kvgb = 6kDv d 5

2π Di ln(R/Rid )

= zid Di

Kid =

Dv = ln(R/Rvd ) 1 + zvd 2π

= zvd Dv

Kvd =

2π Dv ln(R/Rvd )

4π RDi a 1+ R

=

4π RDv a 1+ R

=

4π R2 Di a = 4π RDi

KiV =

4π R2 Dv a = 4π RDv

KvV =

K2v =

z2v Ω Dv a2 z2i Ω Di K2i = a2 ziv Ω Di Kiv = a2

Rate constant

Table 5.2. Reaction rate constants for defect–sink reactions

2πρd ln(R/Rvd )

4π RρV a 1+ R 2 = kid

> 10−3 cm

= 4π RCP ρCPYv ,

= 6k/d, d 2 kvCP

2 kgb

2πρd ln(R/Rid )

= 4π RCP ρCPYi

ρd = ln(R/Rid ) 1 + zid 2π

= zid ρd

2 kiCP

2 = 24/d 2 , d < 10−3 cm kgb

ρd = ln(R/Rvd ) 1 + zvd 2π

= zvd ρd

2 = kvd

=

2 = kV

Eq. (5.117)

Eq. (5.113)

Eq. (5.112)

Eq. (5.101)

Eq. (5.64)

Eqs. (5.96), (5.97)

Eq. (5.99)

Eq. (5.81)

Eq. (5.62)

Eq. (5.58)

Eq. (5.55)

– –

Eq. (5.55)

Eq. #

–

4π R2 ρV a = 4π RρV

Sink strength

5.8 Coherent Precipitates and Solutes 221

222

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Nomenclature A a C Civ CR Cs D Drad Dth Dm Dy0 y Dx y Em f i v s Jx k kX2 K0 Kgb Kid Kiv Kis Kvd Kvs K2v N riv ris rvs p P2v Px Rd Rid Rvd R2v

Flow rate of defects to sink Lattice constant, grain radius Concentration Interstitial, vacancy concentration Vacancy concentration at void boundary Sink concentration Grain diameter Radiation enhanced diffusion coefficient Thermal diffusion coefficient Ballistic mixing diffusion coefficient Pre-exponential factor in the diffusion coefficient via defect y Diffusion coefficient for species x via y Migration energy of defect y Correlation coefficient Interstitial designation Vacancy designation Sink designation Flux of atom or defect x across a marker plane Boltzmann’s constant Sink strength of sink X Defect production rate Rate constant for defect–grain boundary interaction Rate constant for interstitial–dislocation interaction Vacancy–interstitial recombination rate constant Interstitial–sink reaction rate constant Rate constant for vacancy–dislocation interaction Vacancy–sink reaction rate constant Di-vacancy formation rate constant Atom fraction Vacancy–interstitial recombination radius Interstitial–sink recombination radius Vacancy–sink recombination radius Sink annihilation probability Probability/second of forming a di-vacancy Probability/second that a vacancy jumps to a nearest neighbor to a vacancy Dislocation core radius Reaction rate between interstitials and dislocations Reaction rate between vacancies and dislocations Rate of di-vacancy formation

Problems

R t T Tc ν2 zgb zxy

Radius of unit cell or capture volume surrounding a spherical sink Time Temperature Critical temperature defined by Eq. (5.47) Di-vacancy designation Sink strength for an individual grain boundary Combinatorial number for a reaction between x and y

φ ρd η σs τx ω Ω ξ

Particle flux Dislocation density Parameter defined by Eq. (5.45) Microscopic scattering cross section Time constant for process x Jump frequency Atomic volume Production efficiency term

223

Subscripts a CP d gb i, v m rad R s V

Atoms Coherent precipitate Dislocation Grain boundary Interstitials, vacancies Migration Under irradiation Void radius Sink Void

Superscripts i, v

Interstitials, vacancies

Problems 5.1 Point defect concentration build up during irradiation can be described by: dCv = K0 − KivCiCv − KvsCvCs + ∇ · (Dv ∇Cv ) dt dCi = K0 − KivCiCv − KisCiCs + ∇ · (Di ∇Ci ) dt How do these equations simplify if you are irradiating a single crystal with no defects present? In that case, what is the relationship between vacancy and interstitial concentrations? Do the vacancy and interstitial concentrations differ if you start with a sample that contains defects?

224

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.2 For pure nickel irradiated at 500 ◦C: a) calculate the steady state concentration of vacancies and interstitials. K0 = 5 ×10−4 dpa/s

ΔHmv = 0.82 eV

Cs = 109 cm−3

ΔHmi = 0.12 eV

v i riv = ris = rvs = 10a ΔSm = ΔSm =0

ν = 1013 s−1 b) for a dislocation density of 1012 cm−2 , determine the temperature at which mutual recombination gives way to annealing at fixed sinks. 5.3 A perfect, single crystal Cu wire (cylinder) of radius R = 10 nm and length L R is irradiated at 400 ◦C. The only sink present is the surface. a) Assuming negligible recombination, solve the diffusion equation

∂ Cx = K0 + Dx ∇2Cx ∂t at steady state for x = interstitial or vacancy, to obtain the vacancy and interstitial concentration profiles. What boundary condition do you use at the surface? When you solve the equation, pay attention to the symmetry of the problem to eliminate terms in the expression for ∇2Cx . b) Calculate the rates of absorption (number of defects per unit area and time) at the surface. (Hint: remember that ∇2C is continuous.) 5.4 Calculate the steady state radiation-enhanced diffusion coefficient for copper at T /Tm = 0.5 in terms of K0 , the defect production rate, and ρd , the dislocation sink density. 5.5 Assume for a metal of interest that the interstitial–sink interaction radius and the vacancy–sink interaction radius are equal. Two irradiations are performed at low, but non-negligible sink density. The displacement rate is the same for both irradiations. In the second irradiation, a minor alloying addition doubles the diffusion coefficient of interstitials but does not change the diffusion coefficient for vacancies. By how much does the ratio of the steady state vacancy to interstitial concentrations change? Explain physically what happens to the point defects. 5.6 A sample of aluminum is held at room temperature (20 ◦C) and irradiated with a monoenergetic beam of 1 MeV neutrons at a flux of 1014 n/cm2 s. Assume that the capture radii riv = ris = rvs are all approximately 10a. a) At what sink density does defect annihilation at sinks overtake mutual recombination? b) What is the value of the radiation-enhanced steady state diffusion coefficient of aluminum atoms? How does this compare to the diffusion coefficient in the absence of irradiation? c) Verify that your calculations in part (b) do indeed represent a steady state condition, i.e., dCv / dt = dCi / dt = 0.

Problems

225

5.7 A defect-free Al crystal is irradiated at a displacement rate of 10−5 dpa/s. a) Calculate the steady state concentration of point defects at T = 100 ◦C and 500 ◦C. b) Once steady state is reached, the irradiation is stopped. Calculate the time constant for recombination as a function of temperature. c) One wishes to measure the defect concentration in the irradiated Al, a process assumed to take 100 s. Determine the temperature range for which the defect concentration can be kept within 1% of its value at the end of the irradiation for this length of time. Assume the combinatorial factor, z = 500. 5.8 Following the analysis for the diffusion rate of point defects to spherical sinks, derive an expression for the vacancy concentration profile around a dislocation. What is the vacancy capture rate by dislocations? 5.9 For fcc nickel, determine whether vacancy capture by dislocations is a diffusion-controlled or reaction rate-controlled process. What about interstitial capture by dislocations? zd = Area of the circular region about the dislocation (defined by the capture radius) divided by the number of atoms per unit area rvd = Capture radius for vacancies = 0.6 nm rid = Capture radius for interstitials = 0.7 nm 5.10 It can be shown that the time constant (characteristic time) for the process v+ s → s is t3 = (KvsCs )−1 . At sufficiently high temperature, vacancies may be sufficiently mobile so that the reaction v + v → v2 may terminate the increase in vacancy concentration with time. If the consumption rate of vacancies in di-vacancy formation is KvvCv2 , determine the time constant for the onset of steady state. 5.11 A sample of fcc copper with a low sink density (τ1 < τ2 ) is irradiated at low temperature (T /Tm = 0.3) until steady state is reached. Some time later, all sinks instantly disappear and a new steady state is reached. Determine the magnitude of the change in Cv and Ci between the two steady states. 5.12 Explain the reason (or likely reasons) for the following observations: a) The displacement rate at the surface of a copper sample is 1000 times higher when irradiated with 1 MeV Cu+ ions than with 1 MeV protons at the same flux. b) A scattering experiment using 3 MeV B+ ions on Cu produces yields that disagree sharply with calculations using the Rutherford scattering formula. Why? c) A single crystal of copper is irradiated with 2 MeV He+ ions and the backscatter yield is only 5% of that of a polycrystal. d) Irradiation of a metal with a high neutron flux does not produce a measurable increase in the atom diffusion coefficient. e) Two metals are pressed together and heated to 0.5Tm. It is observed that atoms from the metals intermix at the interface. Attempts to determine the

226

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

defect(s) responsible for the intermixing reveal that vacancies account for 100% of the atom mixing. True or false? Why? 5.13 Two engineers are arguing over how to test the effect of the high point defect concentration developed during irradiation on the deformation rate of nickel at 500 ◦C. Engineer #1 maintains that one can irradiate the sample to the appropriate fluence at the temperature of interest, remove it from the reactor, and heat it back up to temperature to perform the test. Engineer #2 insists that the concentration of point defects decays almost immediately after irradiation ceases and therefore, tests must be performed in situ. Who is right? Why? (Hint: consider the point defect equation for the slowest defect (vacancy) only neglect recombination and consider that the only sinks present are dislocations at a concentration of 109 cm−2 ). ◦ −8 2 DNi v (500 C) ∼ 10 cm /s

a ∼ 0.3 nm 5.14 Assume a solid containing defect sinks is irradiated at a temperature T0 , at which only vacancies are mobile. a) For the case of a high sink density, estimate the time, t1 at which sinks will contribute to vacancy annihilation. Neglect recombination. b) For the case of a low sink density, estimate the time, t2 at which recombination will contribute to vacancy annihilation. Neglect the effect of sinks. c) Describe what changes can be made in either the irradiation process or the material microstructure to force t1 = t2 . Assume a quasi-steady state condition exists, beginning at t1 in part (a) and at t2 in part (b). 5.15 Show that, for a metal with a low sink density undergoing neutron irradiation at low temperature (T /Tm < 0.2), when sinks contribute to interstitial annihilation, the vacancy and interstitial concentrations as a function of time can be written Eq. (5.11) as: Cv = (K0 KisCst/Kiv )1/2 Ci = (K0 /Kiv KisCst)1/2 (Hint: consider this case to be intermediary to the quasi-steady state and steady state cases such that dCi / dt < 0 and dCv / dt > 0 and write the point defect balance equations as inequalities.) 5.16 Two bi-layer samples with a low sink strength are being irradiated at low temperature as part of a radiation-enhanced diffusion experiment. If the displacement rate of the second sample is five times that of the first sample, what is the difference in the radiation-enhanced diffusion coefficient?

References

227

References 1. Rothman SJ (1983) Effects of irradiation and diffusion in metals and alloys. In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, pp 189–211 2. Sizemann R (1978) J Nucl Mater 69/70:386–412 3. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Service, Springfield, VA 4. Lam NQ (1975) J Nucl Mater 56:125–135 5. Wiedersich H (1986) In: Johnson RA, Orlov AN (eds) Physics of Radiation Effects in Crystals. Elsevier Science, New York, p 237 6. Matteson S, Roth J, Nicolet M (1979) Rad Eff 42:217–226 7. Heald PT, Harbottle JE (1977) J Nucl Mater 67:229–233 8. Brailsford AD, Bullough R (1972) J Nucl Mater 44:121–135

Part II

Physical Effects of Radiation Damage

6 Radiation-Induced Segregation

A profound consequence of irradiation at elevated temperature is the spatial redistribution of solute and impurity elements in the metal. This phenomenon leads to enrichment or depletion of alloying elements in regions near surfaces, dislocations, voids, grain boundaries, and phase boundaries. Figure 6.1 shows a plot of solute element profiles across a grain boundary in stainless steel irradiated in a reactor to a dose of several dpa at about 300 ◦C. Note that there is significant depletion of chromium, molybdenum and iron and enrichment of nickel and silicon. Such drastic changes at the grain boundary will cause changes in the local properties of the solid and may induce susceptibility to a host of processes that can degrade the integrity of the component. For this reason, understanding radiation-induced segregation (RIS) is of great importance for reactor performance.

Fig. 6.1. Radiation-induced segregation of Cr, Ni, Si and P at the grain boundary of a 300 series stainless steel irradiated in a light water reactor core to several dpa at ∼ 300 ◦C (after [1])

232

6 Radiation-Induced Segregation

First postulated by Anthony in 1972 [2], and observed by Okamoto and Weidersich in 1973 [3], RIS has its origin in the coupling between defect fluxes and fluxes of alloying elements. Irradiation produces point defects and defect clusters with an approximately random distribution throughout the material. Those defects that are mobile and escape recombination are re-incorporated into the crystal structure at dislocations, grain boundaries and other defect sinks. As shown in Chap. 5, point defects flow to spatially discrete sinks. Since the motion of atoms causes the motion of defects, atom fluxes are associated with defect fluxes. Any preferential association of defects with a particular alloying component and/or preferential participation of a component in defect diffusion will couple a net flux of the alloying element to the defect fluxes. The flux of an element causes its buildup or depletion in the vicinity of defect sinks and, therefore, concentration gradients in initially homogeneous alloy phases. The concentration gradients induce back diffusion of the segregating elements, and a quasi-steady state may be set up during irradiation whenever the defect-driven alloying element fluxes are balanced by diffusion-driven back diffusion.

Fig. 6.2. Schematic of radiation-induced segregation in a binary, 50% A–50% B system showing (a) the development of the vacancy concentration profile by the flow of vacancies to the grain boundary balanced by an equal and opposite flow of A and B atoms, but not necessarily in equal numbers, (b) the development of the interstitial concentration profile by the flow of interstitials to the grain boundary balanced by an equal and flow of A and B atoms migrating as interstitials, but not necessarily in equal numbers, (c) the resulting concentration profiles for A and B

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

233

Figure 6.2 presents a schematic of processes driving segregation in a binary, 50%A–50%B alloy, under irradiation at an elevated temperature. As described in Chap. 5, vacancies and interstitials flow to the grain boundary causing a concentration profile to develop. In the case of vacancies (Fig. 6.2a) the flux of vacancies to the grain boundary is balanced by an equal flux of atoms in the opposite direction. However, if the participation of A atoms in the vacancy flux is larger than the atom fraction in the alloy (and consequently the participation of B atoms is less), then there will be a net loss of A atoms, and a net gain of B atoms at the boundary, giving rise to concentration gradients, such as shown in Fig. 6.2c. Considering interstitials, their flux to the grain boundary is also made up of a flux of A and B atoms. If the participation of B atoms in the interstitial flux is greater than the atom fraction in the alloy (and necessarily, the participation of A atoms in the flux is less than the atom fraction in the alloy) then a net increase in B atoms and a corresponding net decrease in A atoms will result. These processes are shown in Fig. 6.2b. This example shows that both vacancy and interstitial flow to the grain boundary can result in the net accumulation of one alloying element and a corresponding depletion of the other alloying element. Whether element A enriches or depletes when both processes are included depends on the relative strengths of atom association with the respective defect fluxes. In this chapter, we will focus on radiation-induced segregation in concentrated binary and ternary alloy systems and we will explore the dependence of RIS on temperature, dose and dose rate.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys To distinguish a concentrated alloy from a dilute alloy, it will be assumed that a concentrated alloy is one in which the substitutional solute concentration is above a few percent. The following segregation model is also well-suited to describe alloy systems with significant atomic size differences, including the limit in which the undersized component is present in dilute solution. The model for solute segregation as developed by Wiedersich [4] follows. We will consider a binary solid solution of elements A and B which are distributed randomly throughout the solid. Due to irradiation the local vacancy and interstitial concentrations change with time according to the point defect balance equations:

∂ Cv = −∇Jv + K0 − R ∂t ∂ Ci = −∇Ji + K0 − R , ∂t

(6.1)

where −∇Jv and −∇Ji are the divergences of the vacancy and interstitial fluxes, respectively, K0 is the Frenkel pair production rate and R = KivCiCv , is the rate of

234

6 Radiation-Induced Segregation

recombination of vacancies and interstitials. Note also that we have dropped the vector notation for sake of simplicity and thus, we will need to keep track of direction. Equations (6.1) are identical to Eq. (5.1) in the absence of sinks and with the gradient term included. The conservation equations for the alloying elements A and B are:

∂ CA = −∇JA ∂t ∂ CB = −∇JB . ∂t

(6.2)

The defect and atom fluxes in Eqs. (6.1) and (6.2) arise from forces due to chemical potential gradients. In reality, the equations should be solved for chemical potential, but for simplicity, we will use relations between fluxes and concentration gradients. The coupling between atom and defect fluxes is based on simple physical models. Note that in the case of self-ion bombardment, we would also include a production term due to the implanted element concentration. It is assumed that diffusive motions of A and B atoms occur only by vacancy and by interstitial jumps. An important coupling between atom and defect fluxes is that a flux of interstitials drives a flux of A and B atoms, equal in size and direction to that of the interstitials, across any fixed lattice or “marker” plane: Ji = JAi + JBi ,

(6.3)

and, similarly, a flux of vacancies drives a flux of A and B atoms equal in size, but opposite in direction, across the marker plane: Jv = − (JAv + JBv ) .

(6.4)

In Eqs. (6.3) and (6.4) and in subsequent notation, the subscripts indicate the species of flux considered, and superscripts the complementary species by which the flux occurs. In general, the division of vacancy and interstitial fluxes via A and B atoms will not be in the same proportion as the atom fractions in the alloy, NA , NB . That is, vacancies may migrate preferentially via B atoms and interstitials via A atoms, as described earlier and shown in Fig. 6.2. The fluxes of atoms and defects can be expressed in terms of the gradients of the different species by the partial diffusion coefficient: 1 DvA = λv2 zv Nv ωAv fAv , 6

(6.5)

where ωAv is the jump frequency with which an A atom exchanges with a vacancy on a given neighboring site, Nv is the atomic fraction of vacancies, zv is the number of nearest neighbors to the A atom, and λv is the jump distance. The term fAv is the correlation factor for A atoms migrating by vacancies, which accounts for the greater than random probability that after an initial jump, subsequent jumps of the A atom will have a displacement component opposite to that of the initial jump.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

235

In alloys, f is highly composition-dependent and is neglected in the following for simplicity, giving: 1 DvA = λv2 zv Nv ωAv , 6

(6.6)

and the partial diffusion coefficient for vacancies via A atoms is: 1 2 A DA v = λv zv Nv ωv . 6

(6.7)

Note than ωAv = ωvA (= ωAv ) since either jump frequency involves the exchange of a given A atom–vacancy pair. Combining those factors on the RHS of Eqs. (6.6) and (6.7) that are common to both, the diffusivity coefficient is defined as: 1 dAv = λv2 zv ωAv , 6

(6.8)

so that we have: DvA = dAv Nv DA v = dAv NA .

(6.9)

For B atoms, the complementary equations are; DvB = dBv Nv DBv = dBv NB

(6.10)

with 1 dBv = λv2 zv ωBv , 6

(6.11)

where ωBv is the effective exchange-jump frequency of a B atom–vacancy pair that includes a factor accounting for possible binding or repulsion between vacancies and B atoms. The partial diffusion coefficients of A and B atoms via interstitials, and interstitials via the elements, provided migration occurs by an interstitial mechanism, are similarly: 1 DiA = λi2 zi Ni ωAi , 6

(6.12)

which is analogous to Eq. (6.6) We are, however, neglecting the fact that interstitial migration is more complex because more than one atom is significantly involved in any interstitial jump. The partial diffusion coefficients for interstitials are thus: DiA = dAi Ni DA i = dAi NA

(6.13)

236

6 Radiation-Induced Segregation

and DiB = dBi Ni DBi = dBi NB .

(6.14)

The expression for dAi and dBi will depend on the interstitialcy mechanism and will be more complicated than Eqs. (6.8) and (6.11). In writing the partial diffusion coefficients in the form D = dN, we further assume that the spatial dependence resides in the factor N, whereas the ds are composition-independent. The “average” or “total” diffusion coefficients for the various species are Dv = dAv NA + dBv NB Di = dAi NA + dBi NB

(6.15)

DA = dAv Nv + dAi Ni DB = dBv Nv + dBi Ni .

(6.16)

Using the partial and total diffusion coefficients we can write the fluxes of atoms and defects with respect to a coordinate system fixed on the crystal lattice: JA = −DA χ ∇CA + dAv NA ∇Cv − dAi NA ∇Ci JB = −DB χ ∇CB + dBv NB ∇Cv − dBi NB ∇Ci

(6.17)

Jv = dAv Nv χ ∇CA + dBvNv χ ∇CB − Dv ∇Cv = (dAv − dBv ) Nv χ ∇CA − Dv ∇Cv Ji = −dAi Ni χ ∇CA − dBi Ni χ ∇CB − Di ∇Ci

(6.18)

= − (dAi − dBi ) Ni χ ∇CA − Di ∇Ci ∂ ln γA ∂ ln γB where χ = 1 + = 1+ , accounts for the difference between ∂ ln NA ∂ ln NB the chemical potential gradient (the true driving force for the diffusion of A and B atoms) and the concentration gradient, and γA and γB are activity coefficients. The second equality in the expressions for Jv and Ji is obtained by neglecting small perturbations arising from the presence of defects, so that ∇CB = −∇CA . This equality describes the Kirkendall effect from the vacancy and interstitial mechanisms, respectively. That is, the difference in the A atom and B atom fluxes in opposite directions past a marker plane must be made up by an appropriate defect flux. Of the four flux equations, Eq. (6.17) to Eq. (6.18), only three are independent because atom fluxes and defect fluxes through a marker plane must balance: JA + JB = −Jv + Ji .

(6.19)

To obtain the atom and defect distributions in time and space, the set of coupled partial differential equations in Eq. (6.1) must be solved for the appropriate initial and boundary conditions. Inserting the fluxes given in Eq. (6.17) to Eq. (6.19) into

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

237

Eq. (6.1) gives:

∂ Cv = ∇ [− (dAv − dBv ) χΩ Cv ∇CA + Dv ∇Cv ] + K0 − R ∂t ∂ Ci = ∇ [(dAi − dBi) χΩ Ci ∇CA + Di ∇Ci ] + K0 − R ∂t ∂ CA = ∇ [DA χ ∇CA + Ω CA (dAi ∇Ci − dAv ∇Cv )] . ∂t

(6.20)

Note that the terms in brackets are just the fluxes, J, of the respective species. The atomic fractions, N have been corrected to volume concentration according to N = Ω C, where Ω is the average atomic volume of the alloy. The equation for element B is CB = 1 − CA when small defect concentrations are neglected. Assuming that steady state has been reached, we can make some qualitative conclusions about the flux equations in Eq. (6.17) to Eq. (6.19). As steady state: JA = JB = 0 ,

(6.21)

and neglecting defect bias effects in the solid: Ji = Jv ,

(6.22)

since vacancies and interstitials are produced and recombine in equal numbers. Eliminating ∇Ci in the relation for JA in Eq. (6.17) using Eqs. (6.19), (6.21) and (6.22) gives: dAv dAi NA NB dBi dAi ∇CA = − (6.23) ∇Cv . χ (dBi NB DA + dAi NA DB ) dBv dBi Equation (6.23) is a relation between the vacancy concentration gradient and the A atom concentration gradient. It is evident that the relation between the direction of the gradient of alloy component A and that of the vacancy gradient is determined dAi dAv and . Recall from Eqs. (6.8) and by the relative magnitude of the ratios dBv dBi (6.11) that: 1 dAv = λv2 zv ωAv 6 1 2 dBv = λv zv ωBv , 6 and

Av ΔSm ωAv = ν exp k

Av −Em exp kT

,

Bv ΔSm ωBv = ν exp k

Bv −Em exp kT

,

therefore:

Bv Av Em − Em dAv , ≈ exp dBv kT

(6.24)

238

6 Radiation-Induced Segregation

since differences in ΔSm between A and B atoms are small. Similarly: Bi Ai Em − Em dAi ≈ exp . dBi kT

(6.25)

During irradiation, the vacancy concentration always decreases towards a defect dAi > sink, and Eq. (6.23) predicts that the element A becomes enriched at sinks if dBi dAv , i.e., if preferential transport of A atoms via interstitials outweighs preferential dBv transport via vacancies and vice versa. Example 6.1. Segregation in a B–25%A alloy Let us look at a B–25%A alloy (where B = Ni and A = Cu), and assume that there is no preferential association of defects with either A or B atoms. Given the following values for migration energies of the two components via vacancies and interstitials: Av ∼ 0.77 eV Em

Ai Em ∼ 0.10 eV

Bv Em ∼ 1.28 eV

Bv Em ∼ 0.15 eV ,

Then, from Eqs. (6.24) and (6.25) we have: dAv dAi 1.28 − 0.77 0.15 − 0.1 − = exp − exp dBv dBi kT kT 0.51 0.05 = exp − exp kT kT

0

Av − ddAi is positive and the concentration gradient of A follows that Since ddBv Bi of vacancies, we have depletion of A at the sink. If this sink is a free surface, then A is depleted at the surface. If it is a grain boundary, then A is depleted at the grain boundary. More A atoms move away from the sink via vacancies than to the sink via interstitials. Figure 6.3 shows the behavior of the A concentration at a temperature of 500 ◦C and a dose rate of 10−3 dpa/s. Note that the drop in the concentration of A at the sink surface is balanced by a buildup behind the depleted zone. With increasing dose the depleted zone increases in depth and width until back diffusion due to the large concentration gradient causes a leveling off and the establishment of a “steady state” condition at t > 104 s.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

239

Fig. 6.3. Concentration profiles of element A in a B–25%A alloy as a function of irradiation Av = 0.77 eV, time at a temperature of 500 ◦C and for a displacement rate of 10−3 dpa/s; Em Bv Ai Bi Em = 1.28 eV, Em = 0.10 eV, Em = 0.15 eV (after [4])

6.1.1 Solution to the Coupled Partial Differential Equations Solution to the system of partial differential equations given in Eq. (6.20) must be obtained numerically. Solutions can be obtained in either planar geometry (free surface) or spherical geometry (grain boundary). In the Perks code [5], segregation of the alloying elements is modeled adjacent to a plane, which is a perfect sink for point defects, such as a grain boundary or a free surface. Another plane is sufficiently far away to model the conditions in the middle of the grain where there are no concentration gradients. The model calculates the concentrations of the major elements by considering the fluxes of each species caused by the migration of point defects created thermally and by irradiation. Point defect losses occur due to mutual recombination and annihilation at fixed sinks, the boundary surfaces and a uniform and time-independent distribution of dislocations. The detailed radiation-induced microstructure is not considered explicitly, but the sink strength can be adjusted with dose to simulate the buildup of sinks in the microstructure. Once the fluxes are calculated, the divergences can be used to perform the time integration required by the continuity equations in Eq. (6.20). The program calculates the concentration of each species independently. An advantage of this method is that any errors in the calculations are evident when the partial concentrations are summed. The deep boundary condition is representative of the bulk material where there are no concentration gradients for atomic and defect species so that the next flux of each species is always zero. The surface or grain boundary is created as a perfect sink for point defects, thus their concentration at the sink is maintained at their initial values ( dCk / dt = 0). In order to conserve atoms in the solid, the atomic fluxes at the boundary are all zero.

240

6 Radiation-Induced Segregation

6.1.2 Interstitial Binding Undersize solutes can tightly bind to interstitials forming interstitial-solute complexes that migrate as solute interstitials. The RIS model described in Sect. 6.1 can account for solute-interstitial binding by accounting for the non-random occupation of interstitials by A and B atoms in the diffusivity coefficients, dAi and dBi , respectively [4]. The concentrations of A and B interstitials are given as: CA exp(EbAi /kT ) , CA exp(EbAi /kT ) + CB CB , CBi = Ci CA exp(EbAi /kT ) + CB

CAi = Ci

(6.26) (6.27)

where EbAi is the average energy gained by converting a B interstitial into an A interstitial. The term EbAi is referred to as the effective A interstitial binding energy. Clearly, solutes that bind to interstitials will undergo enrichment at sinks by virtue of the flow of interstitials to the sink. Example 6.2. Segregation with interstitial binding in Ni–Si Segregation will occur in systems where strong binding of the interstitials to undersize atoms occurs. Consider the system of B–5%A where B is Ni and A is Si and preferential interstitial association with A atoms occurs. Figure 6.4 shows the calculated concentration profile of alloy component A (Si) for an irradiation temperature of 500 ◦C. Note that element A strongly segregates to the surface. This can be understood by referring to the parameters of Eq. (6.27). Av = E Bv = 1.28 eV and E Ai = 0.9 eV, E Bi = 0.15 eV and We have chosen Em m m m a binding energy of EbAi = 1.0 eV so that:

dAv dAi Ai Bi /kT < 0 − = 1 − exp EbAi − Emi + Em dBv dBi and from Eq. (6.23) the surface becomes strongly enriched in Si. The binding energy in part results from the size difference between Ni and Si. Here the solute atom, Si is considerably smaller and is expected to segregate to the surface according to the argument given in Sect. 6.1.3. Results are supported by the preceding calculation and confirmed by experiment. Figure 6.5 shows that segregation of silicon to the surface does indeed occur in a Ni–1%Si alloy irradiated at moderate temperature. It should also be noted that in the Ni– Si system, the solubility limit for Si is ∼ 10 at%, and that segregation of Si to values of above the solubility limit will result in precipitation of Ni3 Si. Hence one important result of irradiation-induced segregation is that it can lead to local solute concentration that exceeds the solubility limit and results in precipitation. Irradiation can also act to stabilize a second phase that would otherwise not be present in thermodynamic equilibrium and vice versa. These processes are discussed in Chap. 9.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

241

Fig. 6.4. Concentration profiles of element A in a B–5%A alloy as a function of irradiaAv = E Bv = tion time at temperature of 500 ◦C and for a displacement rate of 10−3 dpa/s; Em m Ai = 0.90 eV, E Bi = 0.15 eV (after [4]) 1.28 eV, EbAi = 1.0 eV, Em m

Fig. 6.5. Measured concentration vs. depth profiles for a Ni–1%Si alloy irradiated to doses between 3.9 and 8.5 dpa at temperatures between 560 and 660 ◦C with 3.5 MeV 58 Ni+ ions at a displacement rate of ∼ 10−3 dpa/s at the sample surface (after [6])

6.1.3 Solute Size Effect Size difference between solute atoms plays a major role in determining the magnitude and direction of segregation [6]. To reduce the strain energy stored in the lat-

242

6 Radiation-Induced Segregation

tice, undersize solute substitutional atoms will preferentially exchange with solvent atoms in interstitial positions, whereas oversize solute atoms will tend to remain on, or return to, substitutional sites. Strain-energy considerations also predict that vacancies will preferentially exchange with oversize solute atoms. During irradiation at elevated temperatures, the fraction of undersize solute atoms migrating as interstitials, or of oversize solute atoms migrating against the vacancy flux, may therefore greatly exceed the fraction of solute in the alloy. In other words, any variation in size between solute and solvent atoms will cause the chemical composition of the irradiation-induced interstitial and vacancy fluxes toward sinks to differ from the chemical composition of the alloy. This disproportionate participation of misfitting solute atoms in the defect fluxes to sinks will cause a redistribution of solute, which will produce an enrichment of undersize solute and a depletion of oversize solute near defect sinks. Since the surface of an irradiated solid serves as an unsaturable sink for both vacancy and interstitial-type defects, concentration gradients will be created near the surface of alloys that contain misfitting solute atoms during irradiation at appropriate temperatures. Table 6.1 shows the volume misfit for several solute–solvent combinations and the predicted and observed direction of segregation under irradiation. Note that positive misfits should result in depletion (−) at sinks while negative misfits should result in enrichment (+) at sinks. Example 6.3. Segregation driven by the size effect in Ni–1%Al An example of the size effect is the Ni–Al system. According to Table 6.1, Al−v will be less than E Ni−v Al is an oversized solute in the Ni lattice, and Em m since the oversize Al atoms will preferentially exchange with vacancies. AcdAv dAi cording to Eqs. (6.24) and (6.25), > and depletion at the surface is dBv dBi predicted. In fact, measurement of the segregation of Al in Ni–1%Al irradiated to 10.3 dpa at 510 ◦C and to 10.7 dpa at 620 ◦C shows strong depletion of Al at the surface followed by redistribution behind the surface (Fig. 6.6). The buildup of Al just below the surface results in an Al concentration that exceeds the solubility limit and induces second phase formation as discussed in detail in Chap. 9.

6.1.4 Effect of Temperature The temperature dependence of RIS is shown in Fig. 6.7 for a B–25% A alloy, as determined by solution of Eq. (6.20). Note that with increasing temperatures, the dAi dAv and decreases with profile flattens. This is because the difference between dBv dBi increasing temperature. Figure 6.8 shows that the steady state concentration at the sink surface passes through a minimum as a function of temperature and can be explained as follows. At high temperatures, a large thermal vacancy concentration

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

243

Table 6.1. Effect of solute size on radiation-induced segregation (from [7, 8, 9]) Solute–solvent

Volume misfit (%)

Predicted direction of segregation

Observed direction of segregation

Pd–Cu Pd–Fe Pd–Mo Pd–Ni Pd–W Al–Ge Al–Si Al–Zn Fe–Cr Mg–Cd Ti–Al Ti–V Ni–Al Ni–Au Ni–Be Ni–Cr Ni–Ge Ni–Mn Ni–Mo Ni–Sb Ni–Si Ni–Ti Cu–Ag Cu–Be Cu–Fe Cu–Ni ∗ SS–Ni ∗ SS–Cr ∗ SS–Si ∗ SS–C ∗ SS–Mn ∗ SS–Mo ∗ SS–Cu

−20 −27 −3 −26 −2 −37 −45 −19 +4 −19 −3 −26 +52 +55 −29 +1 −5 +32 +31 +21 −16 +57 +44 −34 −8 −7 −3 +5 −3 +54 +3 +36 +9

+ + + + + + + + − + + + − − + − + − − − + − − + + + + − + − − − −

+ + + + + + + + − + + + − − + − + − − − + − − + + + + − +

∗

− −

SS refers to 316 stainless steel from [8]

leads to a high diffusion rate of alloying elements as well as to a high defect recombination rate; the latter reduces the defect fluxes to sinks, and hence, the amount of solute segregation, while the former increases the back diffusion of segregated alloying elements. At low temperatures, the vacancy mobility is low, the radiation-induced excess vacancy concentration is correspondingly high so that defect recombination becomes dominant, and hence the defect fluxes to sinks decrease and segregation is

244

6 Radiation-Induced Segregation

Fig. 6.6. Measured concentration vs. depth profiles for a Ni–1%Al alloy irradiated to 10.3 dpa at 510 ◦C and to 10.7 dpa at 620 ◦C with 3.5 MeV 58 Ni+ ions at a displacement rate of ∼ 10−3 dpa/s at the sample surface (after [6])

Fig. 6.7. Steady state concentration profiles of element A as a function of temperature for the same alloy and irradiation conditions as shown in Fig. 6.3 (after [4])

reduced. At intermediate temperatures, the thermal vacancy concentration becomes insignificant and the radiation-induced excess vacancy concentration is relatively low. The defect recombination rate is low, and hence defects migrate predominantly to sinks and significant segregation occurs.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

245

Fig. 6.8. Temperature dependence of grain boundary segregation of Ni, Cr and Fe in a Ni– 18Cr–9Fe alloy irradiated with 3.4 MeV protons at 400 ◦C to 1 dpa and at a displacement rate of 7 ×10−6 dpa/s (after [10])

6.1.5 Effect of Dose Rate Decreasing the dose rate will shift the temperature dependence of RIS to lower temperatures as shown in Fig. 6.9. The shift of the curve toward lower temperatures for lower displacement rates can be explained as follows. At a given temperature, a lower point defect generation rate K0 means the vacancies and interstitials are added to the lattice more slowly, or more widely spaced in time. However, their thermal mobility is unchanged and with the lower numbers of defects in the lattice, the probability of finding a sink vs. recombination is increased. Thus, at a given temperature, lower displacement rates tend to increase the role of the sink over the

Fig. 6.9. Dose rate dependence of grain boundary chromium depletion calculated using the MIK model for RIS (after [11] and [12])

246

6 Radiation-Induced Segregation

role of recombination, resulting in greater segregation. At high temperatures, a lower displacement rate means that irradiation-produced vacancies will have less of an impact, so that their effect on segregation is less than that at higher dose rate and the amount of segregation drops with decreasing dose rate.

6.2 RIS in Ternary Alloys Engineering alloys are rarely simple binary alloys. Most structural alloys contain many solutes, each with a specific role in the properties of the alloy. Because of the significance of structural stainless steels that are predominantly composed of iron, chromium and nickel, we will reproduce the development of the time and spacedependent concentration equations for a ternary alloy under irradiation. The following description is a condensation of that given by Lam et al. [13] for a ternary alloy whose components A, B and C are present in concentrations CA , CB and CC (number of atoms per unit volume). We start by writing the defect fluxes partitioned into those occurring via A, B and C atoms in the alloy according to: Ji = JiA + JiB + JiC Jv = JvA + JvB + JvC ,

(6.28)

where the subscripts indicate the species of flux (interstitial or vacancy) and the superscripts indicate the complementary species by which the flux occurs (atom A, B, or C). The partial interstitial fluxes are in the same direction as the corresponding atom fluxes while the partial vacancy fluxes are in the opposite direction to the atom fluxes: JiA = JAi ; JvA = −JAv ;

JiB = JBi ;

JiC = JCi

JvB = −JBv ;

JvC = −JCv ,

(6.29)

and Eq. (6.25) can be written as: Ji = JAi + JBi + JCi Jv = − (JAv + JBv + JCv ) .

(6.30)

These equations express the coupling between defect and atom fluxes across any fixed lattice plane. As with the defect compositions, the alloy composition in time and space can be described by the conservation equations:

∂ CA = −∇ · JA ∂t ∂ CB = −∇ · JB ∂t ∂ CC = −∇ · JC , ∂t

(6.31)

6.2 RIS in Ternary Alloys

247

where JA , JB and JC are the total fluxes of the alloying elements, which can be partitioned into partial fluxes occurring by vacancies and interstitials: JA = JAv + JAi JB = JBv + JBi JC = JCv + JCi

(6.32) .

The defect and atom fluxes are expressed in terms of the concentration gradients of the different species: Jki (≡ Jik ) = −Dik χ ∇Ck − Dki ∇Ci Jkv (≡ −Jvk ) = −Dvk χ ∇Ck + Dkv ∇Cv ,

(6.33)

where k = A, B or C, χ is the thermodynamic factor which relates the concentration gradient to the chemical potential gradient of atoms (as in Eqs. (6.17) and (6.18)), and Dik Dvk , Dki and Dkv are the partial diffusion coefficients of atoms k by interstitials, and vacancies, and of interstitials and vacancies by atoms, respectively. The partial diffusion coefficients have the form: Dkj = dk j N j Dkj = dk j Nk ,

(6.34)

where j = i or v, N j = Ω C j and Nk = Ω Ck are the atomic fractions of defects and of k atoms, respectively, Ω is the average atomic volume in the alloy, and dk j are the diffusivity coefficients for conjugate atom-defect pairs k j: 1 dk j = λk2 zk ωkeffj . 6

(6.35)

Here λk is the jump distance, zk the coordination number, and ωkeffj the effective jump or exchange frequency of the pair. The total diffusion coefficients for interstitials and vacancies are defined as: Di = ∑ dki Nk k

Dv = ∑ dkv Nk ,

(6.36)

k

and for atoms: Dk = dki Ni + dkvNv .

(6.37)

For alloy systems in which atoms of one alloy component interact with interstitials to form bound atom–interstitial complexes, the non-random occupation of interstitials by A, B, and C atoms is accounted for in the same manner as for a binary alloy system. For preferential A atom–interstitial binding, we have by analogy with Eqs. (6.26) and (6.27):

248

6 Radiation-Induced Segregation

CA exp(EbAi /kT ) , CA exp(EbAi /kT ) + CB + CC CB CBi = Ci , Ai CA exp(Eb /kT ) + CB + CC CC CCi = Ci , Ai CA exp(Eb /kT ) + CB + CC

CAi = Ci

(6.38)

where EbAi is the average energy gained by converting a B interstitial or a C interstitial into an A interstitial. From Eqs. (6.31), (6.33), (6.34), (6.35) and (6.28), the defect and atom fluxes with respect to a coordinate system fixed on the crystal lattice are: Ji = −(dAi − dCi )Ω Ci χ ∇CA − (dBi − dCi )Ω Ci χ ∇CB − Di ∇Ci Jv = (dAv − dCv)Ω Cv χ ∇CA + (dBv − dCv)Ω Cv χ ∇CB − Dv ∇Cv JA = −DA χ ∇CA + dAv Ω CA ∇Cv − dVi Ω CA ∇Ci JB = −DB χ ∇CB + dBvΩ CB ∇Cv − dVi Ω CB ∇Ci

(6.39)

JC = −DC χ ∇CC + dVv Ω CC ∇Cv − dCi Ω CC ∇Ci . Small perturbations arising from the presence of point defects are neglected so that CA +CB +CC = 1 and ∇CC = −(∇CA + ∇CB ). Of the five fluxes in Eq. (6.39), only four are independent because the defect and atom fluxes across a marker plane must balance: JA + JB + JC = Ji − Jv .

(6.40)

A system of four coupled partial differential equations describing the space and time dependence of the atoms and defects in the solid is determined by substituting the defect and atom fluxes given by Eq. (6.39) into Eqs. (6.31) and (6.1):

∂ Cv ∂t ∂ Ci ∂t ∂ CA ∂t ∂ CB ∂t

= ∇ · [−(dAv − dCv)Ω Cv χ ∇CA −(dBv −dCv )Ω Cv χ ∇CB + Dv ∇Cv ] + K−R = ∇ · [(dAi − dCi )Ω Ci χ ∇CA + (dBi − dCi )Ω Ci χ ∇CB + Di ∇Ci ] + K − R = ∇ · [DA χ ∇CA + Ω CA (dAi ∇Ci − dAv ∇Cv )] = ∇ · [DB χ ∇CB + Ω CB (dBi ∇Ci − dBv∇Cv )] .

(6.41)

Numerical solutions of Eq. (6.41) are obtained for a planar sample under irradiation. The grain boundary is equated to a free surface and the calculations are performed for only a single grain, taking advantage of the symmetry of the problem. The initial conditions are those for thermodynamic equilibrium of the alloy. Conditions at the boundary are defined as follows. At the grain center, all

6.2 RIS in Ternary Alloys

249

concentration gradients are set equal to zero. At the grain boundary, the concentrations of interstitials and vacancies are fixed at their thermal equilibrium values. The grain boundary atom concentrations are determined by the conservation of the numbers of atoms in the specimen. Atom concentrations are assumed to be initially uniform. Parameters used in the calculation of segregation in Fe–Cr–Ni alloys are given in [13] for the Lam model and in [5] for the Perks model. Equations (6.41) can be solved at steady state to provide a relationship between the vacancy gradient and the atom gradient. This relationship is known as a determinant, M and is a function of the concentrations and diffusivities. The determinant for a three-component alloy is determined in the same way as was done for the binary alloy case Eq. (6.23) and is given by [14]:

Mj =

∇C j = ∇Cv

d jvC j Dj

dkiCk d jiC j − Dj k = j Dk

∑

χ∑ k

dkvCk k = j Dk

∑

dkiCk Dk

.

(6.42)

The determinant can be used to help determine the primary mechanism of segregation in Fe–Cr–Ni alloys. Table 6.2 shows the determinant calculated for Cr, Fe, and Ni for a total of seven alloys assuming that preferential coupling with the vacancy flux causes the segregation, i.e., setting the interstitial diffusion coefficients for Cr, Fe, and Ni to be equal to each other. The segregation trends (enrichment or depletion at the grain boundary) for Cr, Fe, and Ni that were measured on the grain boundaries of these alloys by Auger electron spectroscopy (AES) and energy dispersive spectroscopy in scanning transmission electron microscopy (STEM/EDS) are also listed. For each alloy where the determinant for the element is positive, depletion occurs; where the determinant is negative enrichment occurs. Note that for each element in each of the seven alloys studied, the sign of the determinant agrees with the measurement (by either STEM/EDS or AES) and calculation. This example also shows that while chromium always depletes and nickel always enriches, iron can either enrich or deplete depending on the relative concentrations of nickel and chromium. Table 6.2. Segregation behavior in Ni–Cr–Fe and Fe–Cr–Ni alloys compared to inverse Kirkendall predictions. Determinants (M) calculated using Eq. (6.42) Alloy

MCr MFe

MNi

Ref. Cr

Fe

Ni

Analysis method

Ni–18Cr Ni–18Cr–9Fe Fe–16Cr–24Ni Fe–20Cr–24Ni Fe–24Cr–24Ni Fe–24Cr–19Ni Fe–20Cr–9Ni

3.9 5.0 4.0 5.0 6.3 6.5 5.0

−3.9 −5.4 −7.6 −7.4 −8.5 −4.7 −2.0

[14] [15] [16] [16] [16] [16] [16]

— Depletes Depletes Depletes Depletes Enriches Enriches

Enriches Enriches Enriches Enriches Enriches Enriches Enriches

AES&STEM/EDS AES&STEM/EDS AES AES&STEM/EDS AES AES AES&STEM/EDS

— 0.4 3.6 2.4 1.8 −1.8 −3.0

Depletes Depletes Depletes Depletes Depletes Depletes Depletes

250

6 Radiation-Induced Segregation

In the Fe–Cr–Ni system, Cr is the fast diffuser and Ni is the slow diffuser and Fe is between the two. When the nickel level is high relative to the Cr level, the large amount of enrichment of Ni at the grain boundary cannot be fully compensated by depletion of Cr, so Fe also must deplete. But when the Cr level is high relative to Ni the reverse occurs and Fe enriches. Note that Cr and Ni do not exactly cancel as can be seen in the case of the Fe–24Cr–24Ni alloy in which Ni enrichment is stronger than Cr depletion and Fe must also deplete. This example exposes a key process in RIS, the role of composition in the segregation behavior. When the composition near a sink starts to change, the diffusivities of the elements in that region will change also as diffusion is compositiondependent. The effect of changing local composition needs to be accounted for in order to properly determine the extent of RIS, as will be covered in the next section.

6.3 Effect of Local Composition Changes on RIS We have established that RIS occurs because of differences in the coupling of the various solutes with defects. Further, the difference in the strength of the coupling influences the degree of segregation. Therefore, when the concentration near the sink is significantly different from that in the bulk, the diffusivities of the solutes will change as well, and this change needs to be accounted for in order to accurately determine the composition profile [12]. The Perks model can be modified to include both composition-dependent diffusivities. In the Perks model, the rate of segregation of element k by defect j is described by a diffusivity of the general form given by Eq. (6.24): j kj −Em Sm 2 exp , dkj = 1/6λj zj ν exp k kT or in simplified notation: kj −Em kj dkj = d0 exp , kT

(6.43) kj

where the pre-exponential terms are lumped into a single term, d0 . In most solutions to Eq. (6.41), the migration energies for each element are assumed to be equal, with differences in segregation rates arising from differences in the pre-exponential factors. To account for diffusion in a solution of varying composition, the migration energy term in the exponential must be described as a function of composition [11, 15, 16] as presented in the following paragraphs. For an atom to migrate (Cr migrating in a Fe–Cr–Ni lattice will be used as an example), it must move fromits equilibrium position in the lattice (with equilibrium kj −Em kj ) and travel through a position of maximum potential energy dkj = d0 exp kT

6.3 Effect of Local Composition Changes on RIS

251

Fig. 6.10. Determination of the migration energy for an atom–vacancy exchange in an Fe– Cr–Ni alloy (after [12])

kj −Em (known as the saddle point, with saddle point energy dkj = ), bekT fore moving to a new lattice site. This relationship between the energies is shown schematically in Fig. 6.10. For atom – vacancy exchnge the migration energy is the difference between the saddle point energy and the equilibrium energy: kj d0 exp

Cr-v Cr Cr = ESFe-Cr-Ni − Eeq . Em

(6.44)

In a simple model, the equilibrium energy can be described as the interaction energy between nearest neighbors: Cr-v Eeq = Z [CCr ECrCr + CNi ENiCr + CFe EFeCr + Cv ECr-v ] ,

(6.45)

where Z is the number of nearest neighbors, C is the atomic concentration of atoms and/or defects, and Ekj is the pair interaction energy between an atom k and an atom or vacancy j. Pair interaction energies between unlike neighbors are defined to be a linear average of the like atom pair energies minus any ordering energy: ENiCr =

ENiNi + ECrCr ord − ENiCr . 2

(6.46)

Combining Eq. (6.44) to Eq. (6.46) and requiring that CFe + CCr + CNi = 1, the migration energy for Cr, Ni and Fe via vacancies can be expressed as:

1 CNi CFe Cr-v Em (C E E = ESCr − Z + 1) E + + + C E FeFe v Cr CrCr NiNi Cr-v Fe–Cr–Ni 2 2 2 ord ord + ZCNi ENiCr + ZCFe EFeCr (6.47a)

1 CCr CFe Ni-v Em (C E E = ESNi − Z + 1) E + + + C E FeFe v Ni-v Ni NiNi CrCr Fe-Cr-Ni 2 2 2 ord ord + ZCFe EFeNi + ZCCr ENiCr

(6.47b)

252

6 Radiation-Induced Segregation

Fe-v Em = ESFe Fe-Cr-Ni − Z

1 CCr CFe (CFe + 1) EFeFe + ECrCr + ENiNiFe-v + Cv ENi-v 2 2 2

ord ord + ZCFe EFeCr + ZCNi EFeNi

(6.47c)

In order to determine the migration energies in Eq. (6.47), pair interaction energies and saddle point energies must be calculated. For like atoms, the pair interaction energy is the cohesive energy, Ecoh divided by the number of nearest neighbor bond pairs: Cr ECrCr = Ecoh /(Z/2) ,

(6.48a)

Fe EFeFe = Ecoh /(Z/2) , Ni ENiNi = Ecoh /(Z/2) .

(6.48b) (6.48c)

Since pure Fe and pure Cr occur in the bcc structure, the energy required to convert Fe and Cr to the fcc structure for application to stainless steels must be included in the determination of ECrCr and EFeFe to properly describe the equilibrium energy: f cc f cc bcc ECrCr = ECrCr + ΔGbcc→ , Cr

(6.49a)

f cc EFeFe

(6.49b)

f cc bcc = EFeFe + ΔGbcc→ Fe

.

Pair interaction energies between unlike atoms are determined from the average value of the like-atom pair energies less any ordering energy: (ENiNi + ECrCr ) ord − ENiCr , 2 (EFeFe + ECrCr ) ord − EFeCr EFeCr = , 2 (EFeFe + ENiNi ) ord − EFeNi EFeNi = . 2 ENiCr =

(6.50a) (6.50b) (6.50c)

Finally, the pair interaction energy for atoms and vacancies is fitted to the formation energy of the pure metal and is given by: Cr Ecoh + EfCr-v ECr-v = , (6.51a) Z Ni Ecoh + EfNi-v ENi-v = , (6.51b) Z Fe Ecoh + EfFe-v EFe-v = , (6.51c) Z where Efk-v is the vacancy formation energy in pure k. The last quantity remaining to be determined is the saddle point energy, which is calculated using the saddle point energy of pure Fe, Cr, and Ni. The saddle point

6.4 Effect of Solutes on RIS

253

energy in the pure metal is calculated to reproduce the vacancy migration energy in the pure metal. For example, assuming that in pure Cr both an atom and a vacancy are extracted and placed at a saddle point, then the energy to extract the Cr atom is given by: ECr = Z(CCr ECrCr + Cv ECr-v ) .

(6.52)

The energy to extract the vacancy is: Ev = Z(Cv Evv + CCr ECr-v )

(6.53)

Since CCr +Cv = 1 in a pure metal and since Cv CCr , the sum of ECr +Ev becomes: ECr + Ev = Z(ECrCr + ECr-v ) .

(6.54)

Equation (6.54) represents the equilibrium energy for pure Cr. We want to place the atom at a saddle point with an energy such that: Cr-v Cr Cr = ESpure − (ECr + Ev) = ESpure − Z(ECrCr + ECr-v ) . Em

(6.55)

The saddle point energy in the pure metal is then given as: Cr Cr-v ESpure = Em + Z(ECrCr + ECr-v ) .

(6.56)

This approach, described in the modified inverse Kirkendall (Perks) model called the MIK model [12], was used to model RIS and results were compared to measurements taken on a range of Fe-base and Ni-base austenitic alloys irradiated at temperatures from 200 to 600 ◦C and at doses up to 3 dpa. The RIS results shown in Fig. 6.11 clearly demonstrate the importance of accounting for composition changes near the sinks in the determination of the RIS composition profiles. The MIK model calculations agree with AES measurements of grain boundary nickel concentration in irradiated Fe–20Cr–24Ni much better than the original Perks model. Also, over a range of alloys, doses and irradiation temperatures (Fig. 6.12) the inclusion of local composition changes on RIS results in much better agreement with the data. These data also serve to illustrate the importance of vacancies in RIS in Fe–Cr–Ni alloys at intermediate temperatures. The MIK model calculations did not include either interstitial binding (that is, Ebik = 0) or preferential participation of any of the alloying elements in the interstitial flux. Excellent agreement between model and measurement is achieved solely by preferential participation of alloying elements in the vacancy flux. Hence, in the Fe–Cr–Ni system, atom migration via vacancies appears to be the dominant mechanism of RIS.

6.4 Effect of Solutes on RIS The presence of impurities in a solid can influence the propensity for RIS at the grain boundary. It has been hypothesized that solutes that are oversized or undersized with

254

6 Radiation-Induced Segregation

Fig. 6.11. The modified inverse Kirkendall (MIK) model result compared to the Perks model result and to measurement showing the importance in accounting for the changing local composition at sinks in RIS. Experiment was conducted on Fe–20Cr–24Ni using 3.2 MeV protons at 400 ◦C and at a displacement rate of 7 ×10−6 dpa/s (after [12])

Fig. 6.12. MIK model applied to several alloys under a range of doses and temperatures and comparison to measurement (after [2])

6.4 Effect of Solutes on RIS

255

respect to the lattice atoms can act as traps for vacancies or interstitials. Trapping of point defects by solutes could increase the fraction of vacancies and interstitials undergoing mutual recombination, thus reducing the fraction flowing to sinks, and hence, the degree of segregation. Mansur and Yoo [17] generalized the point defect balance equations to include point defect trapping. Trapping is accommodated by subtracting and adding terms corresponding to trapping and recombination at traps, and the release of point defects from traps. In addition, equations describing the conservation of the trapped defects are also added. As a result, the point defect balances, from Eq. (6.1), are given as follows: Free vacancies:

∂ Cv = ∇ · Dv ∇Cv + K0 − KivCiCv ∂t + ∑ τvl−1Cvl − Cv ∑ Kil Cil − Cv ∑ κvl (Clt − Cvl − Cil ) − KvCv . l

l

(6.57)

l

Free interstitials:

∂ Ci = ∇ · Di ∇Ci + K0 − KivCiCv ∂t + ∑ τil−1Cil − Ci ∑ Kvl Cvl − Ci ∑ κil (Clt − Cvl − Cil ) − KiCi . l

l

(6.58)

l

In Eqs. (6.57) and (6.58), the summations extend over the l = 1, 2, . . ., n types of traps. Similarly, the following equations apply to each of the l = 1, 2, . . ., n types of traps. Traps (concentration in general is a function of position and time):

∂ Clt = fl (r,t) . ∂t

(6.59)

Trapped vacancies: t ∂ Cvl = Cv κvl (Clt − Cvl − Cil ) − τvl−1Cvl − Ci Kvl Cvl . ∂t

(6.60)

Trapped interstitials:

∂ Cilt = Ci κil (Clt − Cvl − Cil ) − τil−1Cil − Cv Kil Cil . ∂t

(6.61)

In Eqs. (6.57) and (6.58), the first three terms are the same as in Eq. (6.1). The remaining terms have the following meaning. Referring to the equation for free vacancies, the fourth term is the release of trapped vacancies from the sink and the variable τvl−1 is the mean time that the vacancy is trapped at the lth trapping site. The mean trapping time is denoted by τ jl = (b2 /D0j ) exp[(Ebjl + Emj )/kT ], where j denotes i j

or v, D0j is the pre-exponential of the diffusion coefficient [D j = D0j exp(−Em /kT )], b is the order of atomic distance, Ebjl is the binding energy of the point defect at

256

6 Radiation-Induced Segregation j

the lth type trap, and Em is the point defect migration energy. The fifth term is the recombination rate of vacancies with trapped interstitials, where Kil is the recombination rate constant for that reaction and is given by Kil = 4π ril Dv or Kvl = 4π rvl Di , where ril and rvl denote the respective radii of the recombination volumes. The sixth term describes the trapping of free vacancies at a trap of type l. The concentration − C ) accounts for the fact that the fraction C /Ct + C /Ct difference (Clt − Cvl il vl il l l traps of type l are already occupied by vacancies and interstitials and hence, are not available as traps for free defects. It also accounts for the fact that a given trap may have a binding energy for both vacancies and interstitials but would not trap both simultaneously, since when one is trapped, the site is then a recombination center. D and κ = 4π r D denote the capture coefficients similar to The terms κvl = 4π rvl v il il i and r are the capture radii of the trap type l recombination coefficients, and the rvl il for the respective point defects. Finally, the seventh term is the loss of defects to all internal sinks and Kv describes the rate constant for all sinks. Equation (6.57) through Eq. (6.61) are substituted for the vacancy and interstitial concentrations in Eq. (6.41) and solved in the same manner as before in a version of the MIK code designated MIK-T. The results of trapping in Fe–16Cr–13Ni containing an oversized solute concentration of 1% is shown in the plot of grain boundary chromium content vs. dose for the case of irradiation at a dose rate of 10−5 dpa/s at a temperature of 400 ◦C and for interstitial and vacancy binding energies up 1.0 eV (Fig. 6.13a). Note that high binding energies on the order 1.0 eV are required for trapping to reduce the amount of RIS. The main effect is a reduction in the amount of grain boundary Cr depletion, but a secondary effect is a slowing of the rate of segregation with dose. Figure 6.13b shows that trapping moves the temperature at which RIS is a maximum to a slightly lower temperature. Figure 6.14 shows the effect of oversize solute addition on grain boundary chromium depletion and nickel enrichment in Fe–Cr–Ni alloys irradiated with protons, and that experimental results qualitatively follow those of the model. As successful as these models are in predicting the direction and magnitude of segregation, they are very incomplete. The models have been developed for binary and ternary systems only, whereas real engineering alloys may contain 10–20 alloying elements. Even though some may be present in very small quantities, they can exert a very large influence on the behavior of the alloy. The Perks and MIK models apply only to solute atoms and not to small interstitial atoms such as B, C and N. Further, many of the thermodynamic parameters required for accurate simulation of RIS are unknown and must be estimated, introducing uncertainty into the results. Despite these shortcomings, they can serve to rationalize to RIS in real systems.

6.5 Examples of RIS in Austenitic Alloys As stated earlier, RIS is an extremely important problem in structural materials exposed to irradiation at elevated temperatures. The changes in grain boundary composition can give rise to microstructure changes (precipitation, dislocation loop structure, void structure) in addition to changes in susceptibility to processes such as

6.5 Examples of RIS in Austenitic Alloys

257

Fig. 6.13. Calculated grain boundary Cr composition (a) as a function of binding energy for the MIK-T model at 400 ◦C and 1 ×10−5 dpa/s for Fe–16Cr–13Ni, and (b) as a function of temperature at a constant dose rate of 10−5 dpa/s at 3 dpa. Percent difference calculated by (MIK-T – MIK)/MIK∗ 100% (after [18])

258

6 Radiation-Induced Segregation

Fig. 6.14. Grain boundary Cr and Ni composition for reference and oversize impurity-doped Fe–Cr–Ni alloys irradiated at 400 ◦C to 3.0 dpa (Zr) and 2.5 dpa (Hf) (after [18] and [19])

intergranular corrosion and stress corrosion cracking. For example, we determined that Cr always depletes in irradiated stainless steels, and the loss of chromium at grain boundaries could cause an increased susceptibility to intergranular corrosion and intergranular stress corrosion cracking, since chromium provides passivity to the alloy by forming a very thin, protective, Cr2 O3 film. As will be discussed in Chap. 15, with increases in dose above some pseudo-threshold level, the amount of intergranular stress corrosion cracking (IGSCC), measured as the percentage of the fracture surface that displays intergranular facets, increases steeply in slow strain rate tests in 288 ◦C normal water chemistry used in boiling water reactors (BWR). Figure 6.15 shows that the grain boundary Cr content also decreases rapidly with dose due to RIS. The loss of Cr may raise the susceptibility of the alloy to IASCC, although other changes are occurring in the microstructure at the same time. Silicon is also observed to segregate very strongly with dose, as shown in Fig. 6.16 for austenitic stainless steels irradiated at ∼ 288 ◦C. These measurements of high levels of Si were made by STEM/EDS. Due to the spatial resolution limit of this technique, the actual grain boundary level of Si may be underestimated by as much as a factor of 3–5, giving concentrations of over 20% Si at the grain boundary. Since Si is soluble in high-temperature water, it is possible that it could be enhancing dissolution at the grain boundary giving rise to increased rates of intergranular corrosion (IGC) and IGSCC.

6.6 RIS in Ferritic Alloys

259

Fig. 6.15. Dependence of grain boundary chromium concentration on dose for a range of 300 series stainless steels irradiated under various conditions. Note that RIS increases with dose through about 5 dpa after which the change is minimal (after [20]) Fig. 6.16. Grain boundary segregation of silicon in 300 series austenitic alloys irradiated with neutrons or protons to 13 dpa

6.6 RIS in Ferritic Alloys RIS is also of significance in ferritic steels, particularly pressure vessel steels where the grain boundary segregation of interstitial impurities such as P can have significant consequences for grain boundary embrittlement. Compared to austenitic steels, little work has been done on the segregation of alloying elements in ferritic alloys. Segregation models for interstitial impurities are not as well-developed as for sub-

260

6 Radiation-Induced Segregation

stitutional solutes. Faulkner [21] has reviewed the segregation data and mechanisms and suggests that RIS in ferritic steels is by defect–impurity complexes and that site competition by other elements at the boundary plays a significant role determining in the amount of segregation of a particular impurity. Focusing on the behavior of P, it is assumed that migration by self-interstitial phosphorus complexes is fast such that the concentration remains uniform across the grain boundary plane. The maximum grain boundary concentration of phosphorus is given by: ⎡

⎤ j j

Cg exp Eb /kT ⎥

Eb ⎢ ξ K0 F(η ) max i ⎢ ⎥

1+ exp Ef /kT CP = Cg ⎣ , (6.62) Ef ∑ C j exp E j /kT ⎦ ADk2 g b j

where Cg is the total impurity concentration in the grain, Ebj is the binding energy between the point defect, the self-interstitial and the impurity atom, Ef is the interstitial formation energy and Cgj is the concentration of impurity atom, j in the grains. The denominator of the first bracket is the sum of point defect binding energy terms for all of the elements entering into the site competition process. In the second bracket, ξ is the defect production efficiency, F(η ) is a recombination term, K0 is the defect production rate, A is associated with the vibrational entropy of the atoms surrounding the point defect, D is the defect diffusion coefficient, and k2 is the sink efficiency. Following segregation to the boundary, the impurity concentration will be determined by site competition at the boundary where the concentration of phosphorus is given by: CP∗ = CPmax

CgP exp(QP /kT ) Cgj exp(Q j /kT ) + CgP exp(QP /kT )

,

(6.63)

j

where CgP is the concentration of P and Cg is the concentration of the other impurity elements in the grains, and QP and Q j are the solute grain boundary binding energies for P and for the other elements, respectively. The value of CP∗ is the maximum expected segregation at steady state. Before steady state is reached, the grain boundary concentration depends on time according to: √ CP (t) − Cg 4Dct 2 Dc t = 1 − exp erfc , (6.64) CP∗ − Cg α 2d2 αd where Dc is the point defect–impurity complex diffusion coefficient, α is the enrichment ratio and d is the grain boundary width. Experimental measurements of P segregation in ferritic steels are shown in Fig. 6.17. Note that while the P concentration increases with dose, it varies significantly with the specific alloy. This variation is likely due to site competition with other impurities, most important of which is carbon. The A533 B steel shown has a high grain boundary P level because it has a low C content. Figure 6.18 shows the competition between P and C at the grain boundary and the P segregation is highest when the C level is low.

6.6 RIS in Ferritic Alloys

261

Fig. 6.17. Dose dependence of the irradiation-induced change in grain boundary phosphorus monolayer coverage normalized with respect to the bulk atomic phosphorus concentration for C-Mn LWR plates, welds and coarse HAZ structure and VVER base metal and weld. All irradiation temperatures are 275 – 290 ◦C except for the Magnox SAWs, which cover the range 186 – 311 ◦C (after [21])

In the higher Cr alloys such as the 9–12%Cr ferritic-martensitic alloys, the behavior of Cr at the grain boundary is of concern because of the potential for the formation of brittle, chromium-rich phases. While Cr depletes in austenitic alloys, recent results have shown that it enriches in F-M alloys, behaving like an undersize solute [22]. Although this behavior is not yet understood, experiments have indeed shown that enrichment of Cr at the grain boundary can be substantial. Figure 6.19 shows that Cr enriches at the grain boundary of a Fe–9Cr alloy (T91) by almost 5 wt% following irradiation with 2 MeV protons to 10 dpa at 450 ◦C. If such enrichment leads to the formation of Cr-rich phases, grain boundary embrittlement could result.

262

6 Radiation-Induced Segregation

Fig. 6.18. Variation of phosphorus and carbon monolayer coverage at grain boundaries of thermally aged and irradiated ferritic alloys (after [21])

Fig. 6.19. Grain boundary composition of a ferritic-martensitic Fe–9Cr steel containing 0.2%V and irradiated with 2 MeV protons at 450 ◦C to 10 dpa (after [22])

Nomenclature

Nomenclature A Cx CP∗ d dxy d0x D Dyx x Eeq Ebxz Efx xz Em Exy ord Exy x ESalloy f F(η ) i k k2 v s Jx K0 Kxy Mj Nx QS j rxy R x Sm t T z

Term associated with vibrational entropy, see Eq. (6.62) Concentration of specie x Maximum grain boundary segregation of P at steady state in ferritic steels Grain size Partial diffusion coefficient divided by Ny Pre-exponential term for diffusion of specie x Diffusion coefficient Partial diffusion coefficient for migration of x via y Equilibrium energy for specie x Binding energy of specie x to defect z Formation energy of specie x Migration energy of specie x migrating via defect z Interaction energy between species x and y Ordering energy for species x and y Saddle point energy for element x in alloy Correlation coefficient Recombination term in Eq. (6.62) Interstitial designation Boltzmann’s constant Sink efficiency Vacancy designation Sink designation Flux of atom or defect x across a marker plane Defect production rate Reaction rate constant for x and y Determinant for specie j (defined in Eqs. (6.23) and (6.39)) Atom fraction of specie x Grain boundary binding energy for solute j Capture radius for defect x by sink/trap y Recombination rate Entropy of migration for specie x Time Temperature Number of nearest neighbors

α γx κxy λ ω Ω

Enrichment ratio Activity coefficient of specie x Capture coefficient of defect x by sink/trap y Jump distance Jump frequency Atomic volume

263

264

6 Radiation-Induced Segregation

τ ξ

Time constant Defect production efficiency

Subscripts eq f g l m

Equilibrium Formation Impurity Trap type Migration

Superscripts j k ord t

Specie or defect solute Ordering Trap

Acronyms AES BWR F-M IASCC IGSCC IGC IK MIK MIK-T RIS STEM-EDS

Auger electron spectroscopy Boiling water reactor Ferritic-martensitic Irradiation assisted stress corrosion cracking Intergranular stress corrosion cracking Intergranular cracking Inverse Kirkendall Modified inverse Kirkendall Modified inverse Kirkendall-trapping Radiation-induced segregation Scanning transmission electron microscopy-energy dispersive spectrometry

Problems 6.1 A sample of Cu–20%Al is irradiated at 500 ◦C. a) Will aluminum segregate to or from the surface? Explain. (Assume that association of defects with Al and Cu atoms is non-preferential.) b) If there is strong binding (a preferential association) of interstitials to the undersized atom, how would your answer to part (a) change? (Take EbCu-i = 1 eV.) c) Repeat part (a) for T = 100 ◦C. (Here, vacancies are immobile.) 6.2 A Ni–18Cr alloy is irradiated at 400 ◦C. a) The chromium concentration is measured at the grain boundary and is found to deplete. What is the sign of the determinant for chromium?

References

265

b) The bulk concentration of nickel decreases from 82 to 70 wt%. Assuming nothing else changes, what happens to the determinant of chromium? State your assumptions. c) If the diffusion coefficient of chromium vacancies decreases, what happens to the Cr segregation profile? 6.3 An Fe–18Cr–8Ni alloy is irradiated and radiation-induced segregation changes the grain boundary composition. Calculate the Ni and Cr equivalents for the bulk alloy and at the grain boundary assuming ΔCr = −5 and ΔNi = +3. In terms of the Schaeffler diagram, how is the grain boundary area different than the bulk? If an Fe–18Cr–20Ni alloy was irradiated under the same conditions, what changes? 6.4 For the ternary alloy Fe–18Cr–20Ni, determine if iron enriches or depletes during irradiation at 500 ◦C. 6.5 For the Fe–18Cr–20Ni alloy in Problem 6.4, determine the migration enCr-v at the grain boundary when the grain ergy for chromium via vacancies, Em boundary composition is Fe–10Cr–30Ni. Cr Ecoh = −4.10 eV Fe Ecoh = −1.28 eV Ni Ecoh = −4.44 eV

EfCr-v = 1.60 eV EfFe-v = 1.40 eV EfNi-v = 1.79 eV ord = 0.005 eV ENiCr ord = 0.003 eV EFeCr

References 1. Bruemmer SM, Simonen EP, Scott PM, Andresen PL, Was GS, Nelson LJ (1999) J Nucl Mater 274:299–314 2. Anthony TR (1972) In: Corbett JW, Ianniello LC (eds) Radiation-Induced Voids in Metals and Alloys, AEC Symposium Series, Conf-701601, p 630 3. Okamoto PR, Harkness SD, Laidler JJ (1973) ANS Trans 16:70 4. Wiedersich H, Okamoto PR, Lam NQ (1979) J Nucl Mater 83:98–108 5. Perks JM, Marwick AD, English CA (1986) AERE R 12121 (June) 6. Rehn LE, Okamoto PR, Potter DI, Wiedersich H (1978) J Nucl Mater 74:242–251 7. Rehn LE (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier Science, New York, p 17 8. Okamoto PR, Wiedersich H (1974) J Nucl Mater 53:336–345 9. Kornblit L, Ignatiev A (1984) J Nucl Mater 126:77–78 10. Was GS, Allen TR, Busby IT, Gan I, Damcott D, Carter D, Atzmor M, Konik EA (1999) J Nucl Mater 270:96–114

266

6 Radiation-Induced Segregation

11. Was GS, Allen TR (1993) J Nucl Mater 205:332–338 12. Allen TR, Was GS (1998) Acta Metal 46:3697 13. Lam NQ, Kumar A, Wiedersich H (1982) In: Brager HR, Perrin JS (eds) Effects of Radiation on Materials, 11th Conference, ASTM STP 782, American Society for Testing and Materials, pp 985–1007 14. Watanabe S, Takahashi H (1994) J Nucl Mater 208:191 15. Grandjean Y, Bellon P, Martin G (1994) Phys Rev B 50:4228 16. Nastar M, Martin G (1999) Mater Sci Forum 294–296:83 17. Mansur LK, Yoo MH (1978) J Nucl Mater 74:228–241 18. Hackett MJ, Was GS, Simonen EP (2005) J ASTM Int 2(7) 19. Fournier L, Sencer BH, Wang Y, Was GS, Gan J, Bruemmer SM, Simonen EP, Allen TR, Cole JI (2002) In: Proceedings of the 10th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, NACE International, Houston, TX 20. Was GS (2004) Recent developments in understanding irradiation assisted stress corrosion cracking. In: Proceedings of the 11th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, American Nuclear Society, La Grange Park, IL, pp 965–985 21. Faulkner RG, Jones RB, Lu Z, Flewitt PEJ (2005) Phil Mag 85(19):2065–2099 22. Gupta G, Jiao Z, Ham AN, Busby JT, Was GS (2006) J Nucl Mater 351(1–3):162–173

7 Dislocation Microstructure

One of the most profound consequences of irradiation on the microstructure of materials is the formation of dislocation loops. Dislocation loops have a bias for interstitials and thus have a strong impact on the development of the irradiated microstructure. They also influence the deformation behavior and consequently, the ductility and hardening of irradiated materials, as will be discussed in Chap. 12. In this chapter, we will review the origin and character of dislocations, their mobility and multiplication and their stresses, strains and energies. The character of dislocation loops will be examined and models for nucleation and growth will be presented. Finally, the stacking fault tetrahedron will be discussed. For a more in-depth treatment of dislocations, the reader is referred to [1, 2, 3, 4].

7.1 Dislocation Lines The discovery of dislocations in crystals has its origin in the discrepancy between the measured and theoretical stress needed to cause shear in a crystal. Consider the stress required to shear a crystal along a given atomic plane. A shear of one atomic distance requires that atoms above the plane all move one lattice spacing relative to those below (Fig. 7.1). To reach the saddle point, each atom must move horizontally a distance of one atom radius, a. Since the separation of two planes is ∼ 2a, the shear strain at the saddle point is γ ≈ a/2a ∼ 1/2. In a perfectly elastic crystal, the ratio of shear stress to shear strain is the shear modulus: σs =μ. (7.1) γ

Fig. 7.1. Initial position of atoms above and below a slip plane, and the motion of the atoms above the slip plane required to cause slip

268

7 Dislocation Microstructure

For a typical shear modulus of 17 GPa and a shear strain of 1/2, the shear stress from Eq. (7.1) is ∼ 8.5 GPa. However, experiments, for example on magnesium, produce deformation at shear stresses of ∼ 1 MPa, which is different from theory by a factor of 104 ! The reason is the existence of dislocations that provide for much reduced shear stresses in crystals. A dislocation is a line that forms a boundary between a region of the crystal that has slipped and one that has not. The two basic types of dislocations lines are the edge and the screw. In an edge dislocation, atoms over the cut surface are shifted in a direction perpendicular to the dislocation line. An edge dislocation can also be thought of as the insertion of an extra half plane of atoms (Fig. 7.2). In a screw dislocation, the atoms over the cut surface are shifted in a direction parallel to the dislocation line (Fig. 7.3a). The screw dislocation itself is a pole about which a spiral ramp of planes circles (analogous to a parking garage ramp) (Fig. 7.3b). There also exist mixed dislocations in which the shift is neither parallel nor perpendicular to the dislocation line, but at some arbitrary angle. Figure 7.4 shows a mixed dislocation in a crystal in which the dislocation line is curved. Note that the boundary separating slipped and unslipped regions is circular. At point A (front face), the dislocation is of pure edge character. At point B (side face), the dislocation is of pure screw character. In between, the dislocation is mixed with the proportion of screw and edge character varying continuously with distance along the line. Figure 7.5 shows the construction of a mixed dislocation.

Fig. 7.2. An edge dislocation described as an extra half plane of atoms above the slip plane

Fig. 7.3. (a) A screw dislocation formed by a cut and a shift of atoms in a direction parallel to the cut line. (b) A schematic showing the “parking ramp” nature of a screw dislocation in which atom planes spiral about the dislocation line

7.1 Dislocation Lines

269

Fig. 7.4. Curved dislocation line with pure screw character at point A, pure edge character at point B and mixed character along the length of the dislocation

Fig. 7.5. Construction of a dislocation line with mixed character

270

7 Dislocation Microstructure

Fig. 7.6. A perfect dislocation loop in a crystal in which the character of the loop varies with position long the loop

A dislocation line can also be made in the form of a closed loop rather than a line that terminates at the crystal surface. Following Fig. 7.6, we make a cut along ABCD and shift the atoms parallel to the plane and then rejoin them. Note that segments AB and DC have edge character and segments BC and AD have screw character. Segments AB and DC have opposite sign in that one has a half plane above the cut and one has the half plane below it. The same is true with segments BC and AD. This loop is termed a perfect dislocation loop. Now suppose that instead of shifting atoms parallel to the plane as we did in the example of a perfect loop, we fill up the cut with more atoms. The shift of atoms on each side of the cut is perpendicular to the surface. Figure 7.7 shows that by insertion of a disk of atoms into the cut, that every segment of the dislocation loop has pure edge character. This is very different from the perfect loop with edge and screw character. This dislocation loop is called a prismatic or Frank loop. One variation is to remove a disk of atoms from the cut rather than insert an extra plane of atoms. 7.1.1 Dislocation Motion Dislocations can move in two modes: glide and climb. Glide is the motion of a dislocation on its slip plane and is conservative motion in that it requires no long-range mass transport in order to occur. Experiments have shown that the logarithm of the dislocation velocity is proportional to the logarithm of the shear stress causing glide: ln g α ln σs ,

(7.2)

which implies a power law relationship between shear stress and dislocation velocity: m σs g = , (7.3) σD

7.1 Dislocation Lines

271

Fig. 7.7. A Frank dislocation loop formed by insertion of a circular plane of atoms between existing planes in the lattice

where m is the stress exponent (∼ 1.65) and σD is the value of the stress that yields a dislocation velocity of 0.01 m/s [5]. Experiments also show that the logarithm of the dislocation velocity is proportional to the reciprocal of the absolute temperature, T : ln g α

1 , T

(7.4)

leading to the following description of the velocity of a gliding dislocation in terms of stress and temperature: g = f (σ ) exp(−E/kT ) .

(7.5)

When dislocations glide, they displace the crystal above the slip plane relative to that below. Figure 7.8 shows that if an edge dislocation glides to the surface, the result is a step on the surface of magnitude equal to the Burgers vector. Screw dislocations will also produce a step on the surface, but on a face that is perpendicular to the dislocation line (Fig. 7.9). The perfect loop described in the last section will also

272

7 Dislocation Microstructure

Fig. 7.8. Slip produced by movement of edge dislocations to the surface of a crystal

Fig. 7.9. Slip produced by movement of a screw dislocation to the surface of a crystal

result in displacement of the crystal when it reaches the surface. Figure 7.10 shows the displacement of the crystal above the slip plane relative to that below. Note that the displacements are entirely consistent with the character of the dislocation where it intersects the surface as shown in Figs. 7.8 and 7.9. A Frank loop is essentially an edge dislocation. The slip plane for this type of loop is defined by the intersection of the loop edge and the adjacent crystal and consists of a cylindrical surface projecting above and below the plane of the loop. Figure 7.11 shows how surface atoms would be displaced if the loop were to glide to the surface. However, this mode of motion is not energetically favorable and this loop is more likely to move by climb rather than glide. Dislocations also move by a non-conservative process called climb. Climb is an important process for edge dislocations and prismatic loops, since unlike screw dislocations that can glide on any plane containing the dislocation, there is only

Fig. 7.10. Slip produced by movement of a perfect dislocation loop to the surface of a crystal

7.1 Dislocation Lines

273

Fig. 7.11. Slip produced by movement of a Frank loop to the surface of a crystal

one possible slip plane for an edge dislocation to glide. Climb is the extension or recession of the extra half plane of atoms by absorption or emission of a vacancy, absorption of an interstitial atom or emission/absorption of clusters of vacancies or SIAs. Figure 7.12 shows the positive climb of an edge dislocation by absorption of a vacancy at the dislocation core. In order for the edge dislocation to move up one lattice spacing, all of the atoms along the edge (into the paper) must absorb a vacancy. Positive climb results in a decrease in the size of the extra half plane, while negative climb results in the increase in the size of the extra half plane. Positive climb is associated with a compressive strain and will be promoted by a compressive stress component perpendicular to the extra plane. Similarly, a tensile stress applied perpendicular to the extra plan promotes growth of the plane and thus, negative climb. Since they are essentially edge dislocations, Frank loops climb in the same manner, where positive climb results in loop shrinkage and negative climb results in loop growth. Note that there is a fundamental difference between the nature of the stress that produces slip and that which produces climb. Slip occurs as the result of shear stress, and climb occurs as a result of a normal stress. Since climb requires that vacancies move through the lattice either to or away from the extra half plane, the rate of climb will be dependent on both the diffusion coefficient of vacancies and their concentration. In unirradiated solids, this means that climb will be most important at high temperature. However, in irradiated solids, the increased population of vacancies will make climb more important at lower tem-

Fig. 7.12. Positive climb of an edge dislocation by absorption of vacancies at its core

274

7 Dislocation Microstructure

peratures. Further, the elevated concentration of interstitials means that they too can contribute to climb in a direction that is opposite to that of vacancies. 7.1.2 Description of a Dislocation A description of a dislocation consists of the specification of the vector defining the line direction, s and the Burgers vector defining the atom shift, b. The Burgers vector is defined as follows: 1. Define a positive direction, s, along the dislocation line (e.g., into the paper). 2. Construct a plane perpendicular to the dislocation line. 3. Starting in a region of perfect crystal (away from the dislocation core), complete a counterclockwise circuit around the dislocation line (in the plane of the paper) 4. The Burgers vector, b is the vector needed to close the circuit. The rule is shown schematically in Fig. 7.13 for a screw dislocation. Following this convention, the Burgers vector of an edge dislocation is perpendicular to the dislocation line. The Burgers vector of a screw dislocation is parallel to the dislocation line. For an edge dislocation, we can determine the Burgers vector in the following manner. Sighting down the dislocation line (along the positive s direction), we make a counterclockwise circuit around the dislocation. The vector connecting the end point to the origin is the Burgers vector. Figure 7.14 shows an example of the determination of the Burgers vector using the construction rule. (Note that it does not matter which direction is called positive, but we need to adopt a convention in order to determine the orientation of the line and the extra half plane in the crystal. If we sighted in the opposite direction, b will be in the opposite direction. What matters is the specification of s relative to b.) Following the convention, Fig. 7.15a shows a dislocation with line direction, s pointing into the paper and b pointing to the left. The dislocation in Fig. 7.15b is identical to that in Fig. 7.15a since the relationship between s and b is the same. However, the dislocation shown in Fig. 7.15c is of opposite sign. For a screw dislocation, we consider a left handed screw (counterclockwise rotation; see Fig. 7.16). With this convention, s and b are in the same direction. Figure 7.17a shows a screw dislocation with Burgers vector in the same direction as s.

Fig. 7.13. Convention for finding the Burgers vector of a dislocation line characterized by direction s

7.1 Dislocation Lines

275

Fig. 7.14. The Burgers circuit for an edge dislocation following the convention shown in Fig. 7.13

Fig. 7.15. Examples of identical edge dislocations (a) and (b) and an edge dislocation of opposite sign (c)

Fig. 7.16. The Burgers circuit for a screw dislocation following the convention shown in Fig. 7.13

The dislocation shown in Fig. 7.17b is identical to that in Fig. 7.17a, but the dislocation shown in Fig. 7.17c is of opposite sign as the other two. An edge dislocation glides in the direction of its Burgers vector. A screw dislocation glides in a direction perpendicular to its Burgers vector. We adopt the following convention to determine the direction of motion of a dislocation line: The positive direction of motion is obtained by a counterclockwise rotation on a plane parallel

276

7 Dislocation Microstructure

Fig. 7.17. Examples of identical screw dislocations (a) and (b), and a screw dislocation of opposite sign (c)

to the slip plane, and through 90◦ from the positive direction of the dislocation line itself. The rule is shown by the illustration in Fig. 7.18a. Figures 7.18b,c show the positive direction of motion for an edge and screw dislocation, respectively. Figure 7.19 shows the direction of motion for a dislocation loop that is characterized by a single Burgers vector (perfect loop) and changes character along the dislocation line. 7.1.3 Displacements, Strains and Stresses Dislocations interact with each other and with other microstructure features through their stress fields. Therefore, it is important to establish the stress and strain fields around a dislocation as well as the energy associated with the dislocation line. We will begin with the screw dislocation and then treat the edge dislocation. Recall the orientation of the screw dislocation is one in which the Burgers vector is parallel to the dislocation line, which means that the displacement of atoms is in the direction of the dislocation line. If we describe the dislocation in cylindrical coordinates, Fig. 7.20, then there is no displacement along the r or θ directions so that: ur = uθ = 0 .

(7.6)

In Cartesian coordinates, the displacement in the x–y plane is zero. The only displacement is in the z-direction, and from inspection, we have in cylindrical coordinates: uz =

b θ, 2π

ur = uθ = 0 ,

(7.7)

and in Cartesian coordinates: uz =

y b tan−1 , 2π x

(7.8)

where b is the magnitude of the Burgers vector. From elasticity theory, we can calculate the strain from the displacement as: 1 εθ z = r

∂ uz ∂θ

=

b , 2π r

εrr = εθ θ = εzz = εrθ = εrz = 0 ,

(7.9)

7.1 Dislocation Lines

277

Fig. 7.18. (a) Rule for determination of the direction of motion of a dislocation on its slip plane and examples of the positive direction of motion for (b) edge and (c) screw dislocations

and in Cartesian coordinates: y b b sin θ = 2 π x2 + y2 2 π r x b b εyz = − cos θ =− 2 π x2 + y2 2π r εxx = εyy = εzz = εxy = 0 .

εxz =

(7.10)

278

7 Dislocation Microstructure Fig. 7.19. Positive direction of motion of a perfect loop characterized by a single Burgers vector

Fig. 7.20. Screw dislocation in the Cartesian coordinate system

The stress field of the screw dislocation is determined from the relation between stress and strain: μb , σrr = σθ θ = σzz = σrθ = σrz = 0 , σθ z = μεθ z = (7.11) 2π r and: μb y μb sin θ σxz = = 2 π x2 + y2 2π r μb x μb (7.12) σyz = − cos θ =− 2 2 2π x + y 2π r σxx = σyy = σzz = σxy = 0 . For an edge dislocation as shown in Fig. 7.21, the displacement of atoms is in the x-direction. The displacement is not so simple here, but we know that the dislocation will be similar at any point along the z-axis and hence, the stress state is one of plane stress. The displacement field around the edge dislocation in Cartesian coordinates is:

λ + μ xy b −1 y ux = + tan 2π x λ + 2 μ x2 + y2

−μ x2 + y2 λ +μ y2 b (7.13) uy = log + 2π 2(λ + 2μ ) c λ + 2 μ x2 + y2 uz = 0 ,

7.1 Dislocation Lines

279

Fig. 7.21. Edge dislocation in the Cartesian coordinate system

where the constant c is added to make the log term dimensionless, but is irrelevant since stresses and strains are derivatives of the displacements. The resulting strains are:

εxx = − εyy =

by μ y2 + (2λ + 3μ )x2 2π (λ + 2μ )(x2 + y2 )2

by (2λ + μ )x2 − μ y2 2π (λ + 2μ )(x2 + y2 )2

(7.14)

x(x2 − y2 )

b 2π (1 − ν ) (x2 + y2 )2 εzz = εxz = εyz = 0 ,

εxy =

where ν is Poisson’s ratio, λ is the Lam´e constant and ν = around an edge dislocation are then:

σxx =

λ . The stresses 2(λ + μ )

−μ b y(3x2 + y2 ) −μ b sin θ (2 + cos2θ ) = 2π (1 − ν ) (x2 + y2 )2 π (1 − ν )r

y(x2 − y2) μb μb sin θ cos 2θ = 2π (1 − ν ) (x2 + y2)2 π (1 − ν )r μb μb x(x2 − y2 ) cos θ cos 2θ = σxy = − 2π (1 − ν ) (x2 + y2 )2 π (1 − ν )r −2 μν b μν by = sin θ σzz = v(σxx + σyy ) = π (1 − ν )(x2 + y2 ) π (1 − ν )r σxz = σyz = 0 .

σyy =

(7.15)

280

7 Dislocation Microstructure

The stresses in cylindrical coordinates are: sin θ μb 2π (1 − ν ) r −μ b cos θ σrθ = 2π (1 − ν ) r −μν b sin θ σzz = 2π (1 − ν ) r σθ z = σrz = 0 .

σrr = σθ θ =

(7.16)

7.1.4 Energy of a Dislocation Energy is stored in any elastic medium that is stressed. Applying a tensile stress to a rod produces a tensile strain, which is proportional to the stress in an elastic solid. Consider a unit cube within the rod. A stress, σ is the total force applied across a face of the cube. The strain is the fractional distance the cube elongates in the direction of the stress. So the work done (energy/unit volume) on the cube is the force times the distance, or: W=

εmax 0

σ dε ,

(7.17)

and from Fig. 7.22, we have: W = 1/2σmaxεmax .

(7.18)

For a generalized stress field, the stored energy per unit volume is: W = 1/2(σxx εxx + σyy εyy + σzz εzz + σxy εxy + σxz εxz + σyz εyz ) ,

(7.19)

and in cylindrical coordinates: W = 1/2(σrr εrr + σθ θ εθ θ + σzz εzz + σrθ εrθ + σrz εrz + σθ z εθ z ) ,

(7.20)

where σi j = σ ji .

Fig. 7.22. Elastic stress-strain curve showing the stored energy in the strain field

7.1 Dislocation Lines

281

Applying Eq. (7.20) to the screw dislocation gives: W = 1/2(σθ z εθ z ) =

μ b2 . 8π 2 r 2

The elastic energy per unit length of the dislocation line is: R R μ b2 R dr μ b2 = W 2π r dr = ln + εc . El = 4 π r 4 π r rc rc c

(7.21)

(7.22)

The limits on the integral are the dislocation core radius, rc , and R. The dislocation core radius is that distance below which linear elasticity does not hold and is generally taken to be several Burgers vectors in magnitude. R is the outer dimension of the crystal, or for polycrystalline materials, R could be taken to be the grain radius. However, a further constraining condition is the presence of other dislocations, which is the case even in a well-annealed metal in which the dislocation density is still ∼ 108 cm−2 . So R is often taken to be the distance midway to the next dislocation. However, the elastic energy is not highly sensitive to R since it appears in the ln term. The term εc is the energy of the dislocation core radius, which is not included in the integral since linear continuum elasticity theory breaks down in this region. Assuming that the stress level in the core is μ /30, then for a dislocation core radius of 5b, the value of εc is approximately μ b2 /10, which is about 10 – 20% of the value of that in the elastic strain field (ln term). For an edge dislocation, the elastic energy per unit length determined in the same way as for the screw dislocation is: R μ b2 ln (7.23) + εc , El = 4π (1 − ν ) rc which is different from the screw dislocation by a factor of (1 − ν ) in the denominator of the first term, or a factor of about 1.6 for ν ∼ 0.3. For typical values of R and rc , μ b2 ≤ El ≤ μ b2 . The elastic energy per unit length of dislocation line is also called 2 μ b2 . the line tension and is denoted by Γ . Generally, Γ is taken to have the value 2 7.1.5 Line Tension of a Dislocation Under a uniform applied shear stress, σs , an element of dislocation line, ds, is displaced in a direction normal to ds by an amount dl (Fig. 7.23). The area swept out by the dislocation line element, ds, is ds dl. The average displacement of the crystal above the slip plane relative to that below is by an element: ds dl dx = b, (7.24) A

282

7 Dislocation Microstructure Fig. 7.23. Dislocation line segment ds sweeping out an area ds dl in the direction of the Burgers vector

where A is the area of the slip plane. The force creating the shear stress is σs A, and the work done is: ds dl dW = F dx = σs A b A (7.25) = σs ds dlb . Since force is work divided by the distance over which it is applied: F=

dW = σs dsb , dl

(7.26)

and the force per unit length is: Fl =

dW / dl = σs b . ds

(7.27)

Consider a curved dislocation line. The line tension produces an inward radial force that tends to straighten out the dislocation line. The dislocation will only remain curved if a shear stress exists to resist the line tension. We wish to determine the shear stress required to maintain the curvature. Consider a segment of a dislocation line as shown in Fig. 7.24. The outward force due to the shear stress is:

σs b ds = 2σs bR dθ .

(7.28)

Fig. 7.24. Inward restraining force on a dislocation line segment ds due to a shear stress σs

7.1 Dislocation Lines

283

The inward restraining force is:

Γ sin( dθ ) ∼ 2Γ dθ .

(7.29)

From Eqs. (7.28) and (7.29) we have the force balance: 2Γ dθ = 2σs bR dθ ,

(7.30)

and solving for σs yields the shear stress in terms of the line tension:

σs =

Γ . bR

(7.31)

For:

Γ≈

μ b2 , 2

then σs =

μb , 2R

(7.32a)

and for

μb . (7.32b) R One mechanism of formation of dislocations in solids is the Frank–Read mechanism. The mechanism is shown in Fig. 7.25 and occurs as follows. A dislocation line segment defined by ABCD and Burgers vector b is such that segments AB and DC are immobile and only segment BC lies in a slip plane. The dislocation segment BC is pinned at the points B and C. The temperature is assumed to be low enough that that climb is not an option. Under an applied stress, the segment BC bows out slightly in response to the stress and adopts the curvature as prescribed by μb the line tension on the dislocation given in Eq. (7.32b) σs = , and for l = 2R, 2R μb . When the force arising from the curvature of the dislocation line can no σs ≈ l longer balance the force produced by the applied stress, becomes unstable and bows out to adopt the configuration shown in Fig. 7.25c. Note that at this point, the line segments P and P have opposite character and as the dislocation continues to bow out they come in contact with each other and annihilate, leaving a region of perfect crystal and a perfect loop. The applied shear stress will cause the loop to expand and will also start the process of creating a new loop from the same BC segment. This process can continue to occur and one such pinned dislocation can produce many loops and will continue as long as the loops are able to expand away from the source. Figure 7.26 shows a micrograph of a Frank–Reed source in a silicon crystal. Eventually, the back stress caused by the previous loops will produce a retarding force on the source and it will shut down. Back stress due to dislocation pileup is discussed in Chap. 12. Γ ≈ μ b2 ,

then σs =

7.1.6 Forces on a Dislocation Application of a shear stress, σxy , on a solid containing an edge dislocation (Fig. 7.27) produces motion in the +x direction. In moving a dislocation a distance L, the external applied stress will have done an amount of work/unit length of

284

7 Dislocation Microstructure

Fig. 7.25. Frank–Read source for the production of dislocations

Fig. 7.26. Micrograph of a Frank–Read source in a silicon crystal (from [6])

Fig. 7.27. Force on an edge dislocation with character s|001|, b|100| due to a shear stress σxy

7.1 Dislocation Lines

285

dislocation line equal to σxy bL. Then the force is F = σxy b. Note that the force is in the +x direction. For a screw dislocation, application of a shear stress, σyz , results in a force σyz b, where the force is in the +x direction (Fig. 7.28). Application of a shear stress σxz produces a force −σxz b, where the force is in the −y direction, and motion is perpendicular to the slip plane. What if we apply a stress to an edge dislocation that produces a force in a direction perpendicular to the slip plane? A tensile stress, σxx , applied to the edge dislocation in Fig. 7.29 will produce a downward force on the dislocation equal to −σxx b. The only way that the dislocation can respond to this stress is to climb. Forces on mixed dislocations are more complicated. If a dislocation is oriented along the +z-direction and its slip plane is perpendicular to the y-axis, then the Burgers vector can be described by: b = bx i + bz k ,

(7.33)

Fig. 7.28. Force on a screw dislocation with character s|001|, b|001| due to a shear stress σyz

Fig. 7.29. Force on an edge dislocation with character s|001|, b|100| due to a normal stress σxx

286

7 Dislocation Microstructure

where bx and bz are edge and screw components of the Burgers vector and i and k are unit vectors in the x and z-directions, respectively. An external stress placed on the surfaces of a crystal containing a dislocation includes six components; σxx , σyy , σzz , σxy , σxz and σyz . Of these six stress components, only σyz and σxy can exert a force on an edge dislocation that will cause motion in the slip plane. Stress components σxz and σxx causes motion perpendicular to the slip plane. The term σzz does no work, nor does σyy . The total force on a unit length of dislocation line is then: F = (σxy bx + σyz bz )i − (σxx bx + σxz bz )j ,

(7.34)

where the first term is the force component parallel to the slip plane and the second term is the force component normal to the slip plane, and n = (i, j, k) defines the unit vector. As an example of forces between dislocations, let us take the case of parallel screw dislocations. The force, F that a screw dislocation situated at the origin (with Burgers vector b) exerts on a parallel screw dislocation at a position (r, θ ) (with Burgers vector b ) is: F = σyz bz · i − σxz bz · j μ br cos θ μ br sin θ b+ b = 2π r 2 2π r 2 μ bb r = (cos θ · i + sin θ · j) . 2π r 2

(7.35)

The force is in a direction that is perpendicular to the dislocation lines. It is repulsive if the dislocations are of the same sign, and attractive if the dislocations are of opposite sign. The force on the dislocation at the origin due to the dislocation at (r, θ ) is equal in magnitude but opposite in sign from the force on the dislocation at (r, θ ) due to that at the origin. The force components in the xy-plane are shown in Fig. 7.30a and the magnitude of the forces as a function of θ are shown in Fig. 7.30b. A dislocation of mixed character represents the generalized case of a force on a dislocation. For a mixed dislocation, the Burgers vector is: b = bx i + by j + bz k = b1 i + b2 j + b3 k .

(7.36)

Therefore, we write the incremental work done on a dislocation of Burgers vector described by Eq. (7.36) due to an arbitrary stress σi j , as:

δW =

3

∑ bi σi j n j dA ,

(7.37)

i=1 j=1

or in matrix notation: dW = b σ n dA ,

(7.38)

7.1 Dislocation Lines

287

Fig. 7.30. The x and y-components of the force on a screw dislocation due to another dislocation (a) in the x–y plane, and (b) as a function of θ

where σ is the stress tensor, n is the unit vector perpendicular to the slip plane and b is the Burgers vector. Actually, b is a column vector so that Eq. (7.38) is written as: dW = bT σ · n dA .

(7.39)

The term n dA can be written as dA which is just L(s × dl) ,

(7.40)

where s is the unit vector in the direction of the dislocation line, L is the length of the dislocation line and dl (= dxi + dyj + dzk) is the unit vector in the slip plane and is normal to s and n. Recall that b = bx i + by j + bz k, so b has a component only in the direction dl. Since A · B × C = A × B · C, then: dW = bT σ × s · dlL ,

(7.41)

and: 1 dW = bT σ × s · dl . L

(7.42)

288

7 Dislocation Microstructure Fig. 7.31. Orientation of an edge dislocation for the determination of the forces due to a generalized stress field

The term bT σ × s in Eq. (7.42) is the force per unit length on a dislocation due to an external stress which tends to displace the dislocation, and is designated: f = bT σ × s ,

(7.43)

and is known as the Peach–Koehler equation. Let us apply the Peach–Koehler equation to the case of an edge dislocation described vector and direction: Burgers by 0 1 b 0 and s 0 and shown in Fig. 7.31. We write the first quantity in Eq. (7.43) 1 0 as: σxx σxy σxz bT σ = b|100| σyx σyy σyz = b|σxx σxy σxz | , (7.44) σzx σzy σzz and then taking the cross product with s gives: i j k bT σ × s = b σxx σxy σxz . 0 0 1

(7.45)

The cross product, or determinant is bσxy i − bσxx j, and the force on the dislocation is: f = bσxy i − bσxx j .

(7.46)

Note that fx = bσxy is a glide force in the +x-direction and the force component fy = −bσxx is the climb force in the −y-direction. Only σxy and σxx can exert forces on a dislocation with Burgers vector and direction defined as in this example. For with Burgers vector and direction given by: ascrew dislocation 0 0 b 0 and s 0 , and shown in Fig. 7.32, we have: 1 1

7.1 Dislocation Lines

289

Fig. 7.32. Orientation of a screw dislocation for the determination of the forces due to a generalized stress field

σxx σxy σxz bT σ = b|001| σyx σyy σyz = b|σxz σyz σzz | , σzx σzy σzz and then taking the cross product with s gives: i j k f = bT σ × s = b σxz σyz σzz = bσyz i − bσxz j , 0 0 1

(7.47)

(7.48)

and fx = bσyz and fy = −bσxz . Note that only σyz and σxz can exert a force on a dislocation defined in this example. 7.1.7 Interactions Between Dislocations Let us examine interactions between dislocations. We will look at edge–edge, screw–screw, and edge–screw interactions. We will begin with the edge–edge interaction. Edge–edge interaction To find the force on dislocation (2) due to the presence of dislocation (1), we locate dislocation (1) at the origin of our coordinate axes and dislocation (2) at some arbitrary position (Fig. 7.33a). According to the Peach–Koehler equation, the force is: f = b T σ × s , where the Burgers vector and direction are those of disloca(2) (1)

(2)

tion (2), and the stress is due to dislocation (1). The first term in the cross product then becomes: σxx σxy 0 bT σ = b|100| σyx σyy 0 = b|σxx σxy 0|; , (7.49) % &' ( 0 0 σ zz (2) % &' ( (1)

290

7 Dislocation Microstructure

Fig. 7.33. (a) Orientation of dislocations to determine the force on edge dislocation (2) due to edge dislocation (1), and x and y-components of the force (b) in the x–y plane, and (c) as a function of θ

and

i j k f = bT σ × s = b σxx σxy 0 = bσxy i − bσxx j . (2) 0 0 1

(7.50)

The force on dislocation (2) can be written as: F=

μ bb(2) μ bb(2) (cos θ cos2θ )i − sin θ (2 + cos2θ )j , 2π (1 − ν )r 2π (1 − ν )r &' ( % &' ( % Fx (θ )

(7.51)

Fy (θ )

and the force components in the x–y plane are shown in Fig. 7.33b, and as a function of θ in Fig. 7.33c. Note that if dislocation (2) has the same s but the Burgers vector is in the opposite direction, then the net effect on the resultant force is simply a change in sign of

7.1 Dislocation Lines

291

each of the terms in Eq. but preservation of the magnitudes. If dislocation (2) (7.51) 0 has Burgers vector b 1 , then the preceding analysis becomes: 0 σxx T b σ = b|010| σyx % &' ( 0 (2) %

σxy 0 σyy 0 = b|σxy σyy 0| , 0 σzz &' (

(7.52)

(1)

i j k f = bT σ × s = b σxy σyy 0 = bσyy i − bσxy j . (2) 0 0 1

(7.53)

In this case, the x-component of the force produces a positive climb force to the right, and the y-component of the force produces a negative (downward) glide force. Screw–screw interaction For two screw dislocations as shown in Fig. 7.34, the force on dislocation (2) due to dislocation (1) is: i j k (7.54) f = bT σ × s = b σxz σyz 0 = bσyz i − bσxz j , (2) 0 0 1 where the x-component of the force, bσyz is to the right, and the y-component of the force, −bσxz is downward in Fig. 7.34. The force on dislocation (2) can be written as: F=

μ bb(2) cos θ i + sin θ j , 2π r

(7.55)

and the force components in the x–y plane have already been shown in Fig. 7.30a, and as a function of θ in Fig. 7.30b.

Fig. 7.34. Orientation of dislocations to determine the force on screw dislocation (2) due to screw dislocation (1)

292

7 Dislocation Microstructure Fig. 7.35. Orientation of dislocations to determine the force on screw dislocation (2) due to edge dislocation (1)

Edge–screw interaction The last example is the determination of the force between an edge and a screw dislocation as defined in Fig. 7.35. We know that an edge dislocation has no xz or yz stress components, which are needed to move a screw So we can state dislocation. 0 1 the following rules: For an edge dislocation with b 0 and s 0 , the only stresses 1 0 that produce a force on it are σxx and σxy . The stress field around thedislocation has 0 0 components σxx , σyy , σzz and σxy . For a screw dislocation with b 0 and s 0 , the 1 1 only stresses that produce a force on it are σxz and σyz . The stress field around the dislocation has components σxz and σyz . 7.1.8 Extended Dislocations Slip occurs in the fcc lattice on (111) planes and in the 110 direction. The Burgers vector is a/2[110], which is the shortest lattice vector connecting an atom at the cube corner with a neighboring atom at the center of a cube face. However, the atom arrangement on the {111} slip plane is such that slip in the [110] direction is not the easiest path. Figure 7.36a shows the atom arrangement on a close-packed (111) plane. The {111} planes are stacked in the sequence ABC ABC. . . ., such that the centers of the A plane of atoms fall on top of each other, ¯ shown and similarly for the B and C planes of atoms. The vector b1 = a/2[101] in Fig. 7.36a is the observed slip direction. However, if atoms are considered as hard spheres, this direction represents a high-energy path as atoms moving from one B site to another must climb over the A atoms. A simpler path is by way of vectors b2 and b3 , which is along the “valleys” between the A atoms. This dislo¯ → a/6[21¯ 1] ¯ + a/6[112]. ¯ Essencation reaction is given by: b1 → b2 + b3 , a/2[101] tially, the Burgers vector, b1 of the total dislocation has been dissociated into two partial dislocations b2 and b3 . Figure 7.36b shows the atom arrangement of the partial dislocations on the {111} plane and Fig. 7.36c shows the vector diagram

7.1 Dislocation Lines

293

Fig. 7.36. Slip on the close-packed (111) plane in the fcc lattice. (a) Slip directions. (b) Location of atoms in a Shockley partial. (c) Dislocation dissociation into to partial dislocations

of the dissociation of the total dislocation into two partial dislocations. The partials are often called Shockley partials and the combination of the two partials is termed an extended dislocation. Dissociation is independent of dislocation character and the partial dislocations move as a unit that maintains the equilibrium width between them. The space between the partials is referred to as the faulted region or the stacking fault and its size is determined by the stacking fault energy, SFE. The lower the SFE, the greater the separation of the partials and the higher the energy, the closer they are together. Stacking faults are important in cross slip as the partials must recombine in order for cross slip to occur. Ex-

294

7 Dislocation Microstructure

tended dislocations also occur in hcp lattices, but are not commonly observed in bcc metals. 7.1.9 Kinks and Jogs Both edge and screw dislocations can acquire jogs, or steps in the dislocation line by interaction with other dislocations. The jogs are of two types. A jog that lies in the slip plane instead of normal to it is called a kink. Figure 7.37a shows an edge dislocation with a kink of screw character that lies in the slip plane of the edge dislocation, and Fig. 7.37b shows a screw dislocation with a kink of edge orientation. Kinks are unstable as they can line up and annihilate during glide. A second type of jog is shown in Fig. 7.37c in which the jog and the dislocation are of edge orientation. These types of jogs are able to glide since they lie in the slip plane of the dislocation. The only difference between the motion of the jogged edge dislocation and the ordinary edge dislocation is that instead of gliding along a single plane, it glides over a stepped surface. Another type of jog is the most important in plastic deformation and is shown in Fig. 7.37d. This is a screw dislocation containing a job with an edge orientation. The only way the screw dislocation can move to a new position and take its jog with it is by climb of the jog. Figure 7.37e shows the movement of a jogged screw dislocation as the segments between jogs bow out in the slip plane under an applied stress producing a trail of vacancies left behind the jog as the dislocation moves in its slip plane.

7.2 Faulted Loops and Stacking Fault Tetrahedra Because of their importance in irradiated materials, we will discuss Frank loops at greater length. Frank loops are important in irradiated materials because they are often nucleated in a displacement cascade. Recall that the cascade consists of a core of vacancies surrounded by a shell of interstitials (Figs. 3.3 and 3.9). If the vacancy core or the interstitial shell collapse (condense) onto a close-packed plane, Frank loops may be generated. In both cases, a stacking fault results. Vacancy condensation produces an intrinsic fault and interstitial condensation results in an extrinsic stacking fault. The faults are described as follows. In regular, close-packed lattices such as fcc and bcc, atom layers follow a regular stacking sequence. In the fcc lattice, the stacking sequence is ABCABCABC. . . , indicating that every third layer lies over the first layer. Removal of a layer of atoms results in a break or a fault in the stacking sequence. Removal of a plane of atoms produces an intrinsic stacking fault, which is also known as a single fault, and the dislocations attached to the single fault are S-dislocations, giving an S-Frank dislocation (Fig. 7.38a). For example, the sequence is modified to ABCAB/ABCABC. . . , where “/” denotes the fault or missing plane of atoms. Insertion of an extra plane of atoms produces a double fault in the stacking sequence; ABCAB/A/CABC. . . . (Fig. 7.38b). This is an extrinsic or double fault and the dislocations are D-dislocations giving a D-Frank loop. The Burgers vector of the S-Frank

7.2 Faulted Loops and Stacking Fault Tetrahedra

295

Fig. 7.37. Kinks and jogs in dislocations. (a) Edge dislocation with a kink of screw character. (b) Screw dislocation with a kink of edge orientation. (c) Edge jog in an edge dislocation. (d) Edge jog in a screw dislocation and direction of motion of the dislocation. (e) Movement of a jogged screw dislocation of part (d) showing bowing of the segments between jogs and the trail of vacancies left behind the trail of jogs (after [7])

296

7 Dislocation Microstructure

Fig. 7.38. Schematic of an (a) intrinsic stacking fault and an (b) extrinsic stacking fault

and D-Frank loops are identical. Since a Frank loop results from addition or removal of close-packed planes, b must be directed√normal to the (111) plane and has a length equal to the spacing between planes, a/ 3, then the Burgers vector is described by b = a/3[111]. Since it is extremely difficult to move on its slip plane (the glide plane is actually a cylinder defined by the edge of the loop), the Frank loop is considered to be sessile or immobile since its glide plane is a cylinder defined by the projection of the loop perimeter in a direction perpendicular to, and above or below the plane of the loop. A Frank loop can also unfault either autocatalytically or by reaction with a dislocation line to form a perfect loop. This process is described in Chap. 12. Another dislocation configuration that can form in irradiated metals is the stacking fault tetrahedron (SFT). A SFT is a three-dimensional stacking fault configuration that is in the shape of a tetrahedron. SFTs are believed to evolve directly from vacancy clusters produced in cascades. They are also believed to evolve from Frank loops. A Frank loop will always line on a (111) plane in an fcc lattice. Figure 7.39a shows a loop of triangular shape on a (111) plane with edges parallel to [110] directions. A Frank dislocation that is parallel to a [110] direction can lower its energy by splitting into a Shockley dislocation, a/6[211] and a stair-rod dislocation. The slip plane of the Shockley dislocation is also a (111) plane but it is different from that containing the Frank loop. Figure 7.39b shows two of the three Shockley dislocations formed from the three sides of the Frank loop, moving up (111) planes. Each Shockley has left behind it a stair-rod dislo-

7.2 Faulted Loops and Stacking Fault Tetrahedra

297

Fig. 7.39. A stacking fault tetrahedron (SFT) formed by faults on each of the faces of the tetrahedron (after [1])

cation, a/6[110] in the position formerly occupied by a side of the Frank dislocation loop (edge of the triangle). The stacking fault contained in the Frank loop now bends at the stair-rod dislocation and extends up onto the close-packed (111) planes of the Shockley dislocations. As the Shockley dislocations move up the planes shown in Fig. 7.39b, they eventually meet at the intersections of their slip planes and the intersections of Shockley dislocations result in other stair-rod dislocations along the remaining three edges of the tetrahedron. The final configuration is a tetrahedron whose sides are stacking faults and whose edges are stair-rod dislocations (Fig. 7.39c). The Frank dislocation and the Shockley dislocations no longer exist. Dislocations can also interact with SFTs. MD simulation of the interaction of a dissociated a/2[110] dislocation (into two Shockley partials, a/6[121]) on the (111) glide plane shows that several types of interaction are possible [8]. When the SFT is in the slip plane of the dislocation, the SFT may be cut by the dislocation

298

7 Dislocation Microstructure

and recovers by a shift of the structure above the glide plane to regain its original shape. The interaction can also create ledges in the SFT that can reduce stability and lead to dissolution. TEM observations show that SFTs can be cut multiple times by dislocations in channels.

7.3 Defect Clusters As described in Chap. 3, the fraction of defects produced in a cascade is between 20 and 40% of that predicted by the NRT model due to intracascade recombination. Of these, not all appear as single interstitial atoms or isolated vacancies. A significant fraction of defects are created in the form of clusters, rather than as single defects. Vacancy clusters may grow to form voids, which are an important microstructure feature that influences both dimensional (Chap. 8) and mechanical (Chap. 12) properties of materials. If the clusters are stable, they may also migrate away from the cascade region and be absorbed at sinks such as dislocations and grain boundaries. Interstitial and vacancy clusters must be treated separately since in general, interstitial clusters are stable and vacancy clusters are not. Their mobilities differ as well with interstitial clusters exhibiting greater mobility than their vacancy counterparts. 7.3.1 Fraction of Defects Forming Clusters In-cascade clustering of defects is important because it promotes nucleation of extended defects. Interstitial clustering can occur in one of two ways. In the first, interstitial clusters are created in the transition between the collisional and thermal spike phases in which atoms that are displaced from the cascade center due to the initial shock wave are pushed into interstitial locations. Alternatively, clusters can occur during the thermal spike phase by short-range diffusion driven by the elastic interaction between neighboring interstitials. The probability of clustering and the size of the clusters tend to increase with increasing PKA energy and a higher proportion of SIA form clusters than do vacancies [9]. Figure 7.40 shows the fraction of interstitials that form clusters as a function of the PKA energy in several metals and at 100 K, as determined by MD simulation [10]. Note that the clustered fraction increases quickly with T as damage transitions from single displacements to cascade morphology. In contrast to the Frenkel pair production efficiency (Fig. 3.20) the clustered fraction varies with the metal, and while there are only 5 metals shown here, the clustering appears to occur according to the crystal structure with the highest clustering fraction occurring for the fcc structure and the lowest for the bcc structure with the hcp structure in between. While MD results show that the fraction of interstitials in clusters is larger in copper than in α -iron by ∼ 70 to 45% at 100 and 600 K for PKA energies above 5 keV [11], experimental evidence shows that the cluster density in copper is as much as 103 higher than that in Fe [12]. While the size of this difference is not

7.3 Defect Clusters

299

Fig. 7.40. The fraction, ficl , of SIAs that survive as clusters containing at least two interstitials in several metals and Ni3 Al at 100 K (after [10])

understood, it may have its origins in the nature of the cluster as discussed in the next section. Interstitial clustering depends on the irradiation temperature [9, 10, 13]. Figure 7.41 shows that with increasing temperature, the fraction of interstitials in clusters in α -iron decreases for damage energies between 5 and 40 keV. Actually, interstitial clustering increases at higher temperatures due to the more compact nature and longer lifetime of the cascade at higher temperature, providing more time for interstitials to diffuse and interact. Recall from Sect. 3.6 and Fig. 3.21 that the Frenkel pair production decreases slightly with temperature. Combining these results, the effect of temperature can be described as resulting in an increasing fraction of the decreasing population of interstitials forming clusters as the temperature increases, yielding a net decrease in fid .

Fig. 7.41. The fraction of SIA clusters formed in a sessile configuration in α -iron at the end of the thermal spike as a function of PKA energy and irradiation temperature (after [10])

300

7 Dislocation Microstructure

Fig. 7.42. The fraction ficl , of SIAs that survive in clusters of two or more, three or more and four or more in copper at 100 K (after [10])

Finally, the clustered fraction can be broken down according to cluster size to reveal the dependence of clustering on cluster size. Figure 7.42 shows the fraction of SIAs in clusters of sizes 2, 3 and 4 in copper as a function of damage energy for an irradiation temperature of 100 K. Note that the cluster fraction is very sensitive to minimum cluster size, especially at lower damage energies, yielding a net decrease in ficl . Clustering of vacancies occurs within the core of the cascade as well and the extent of clustering varies with the host lattice. Based on measurements of size and number density of vacancy clusters in irradiated metals, the fraction of vacancies in clusters is estimated to be less than 15%. The true fraction may be larger because of the invisibility of small clusters, but also the fact that vacancy clusters are not nearly as stable as interstitial clusters as will be shown in the next section. 7.3.2 Types of Clusters The structure of the cluster is a strong function of the crystal structure [12, 14]. In α -Fe, MD simulation shows that the most stable configuration of small clusters (< 10 SIAs) is a set of 111 crowdions. Next in stability is the 110 crowdion. As the cluster size grows (> 7 SIAs) only two configurations are stable, the 111 and 110 crowdions. These crowdions also may act as nuclei for the formation of

7.3 Defect Clusters

301

Fig. 7.43. Binding energy for SIA loops of different shapes and Burgers vectors (a) in α -Fe, and (b) in copper (after [12])

perfect interstitial dislocation loops with Burgers vector 1/2111 or 100, respectively. In fcc copper, the 100 dumbbell is the stable configuration of the SIA and the smallest cluster is of the form of two 100 dumbbells. Larger clusters can have two configurations: a set of 100 dumbbells or a set of 110 crowdions, each with {111} as the habit plane. During growth, the clusters transform into faulted Frank loops with Burgers vector 1/3111, and perfect loops with Burgers vector 1/2110. The binding energy of SIA loops in Fe and in Cu is shown in Fig. 7.43a,b, respectively. Note that the binding energy for SIA loops in Cu is slightly higher than for SIA loops in α -Fe, in agreement with the higher clustering fraction predicted by MD modeling. Figure 7.44 shows a micrograph of interstitial clusters and small interstitial loops in a copper foil after irradiation with 30 keV Cu+ ions. Note that these defect clusters are only a few nanometers in size. Cluster densities can reach very high levels as shown in Fig. 7.45. The stability of vacancy clusters is low relative to interstitial clusters. The most stable configurations for vacancy clusters in α -Fe are either a set of di-vacancies concentrated on two adjacent {100} planes, or a set of first nearest neighbor vacancies on a {110} plane. During cluster growth, the first type results in a perfect dislocation loop with Burgers vector 100 and the second unfaults into a perfect

302

7 Dislocation Microstructure Fig. 7.44. Micrograph of interstitial clusters and small interstitial loops in copper irradiated with 30 keV Cu+ . Defects are highlighted by the circles on the micrographs (after [15])

Fig. 7.45. Dose dependence of cluster densities measured in α -iron and copper irradiated with fission neutrons at temperatures below 0.3 Tm (after [12])

7.3 Defect Clusters

303

Fig. 7.46. Binding energy of vacancy loops of different shapes and Burgers vectors in (a) α -Fe, and (b) copper (after [12])

loop with Burgers vector 1/2111. Vacancy loops can also exist in the faulted configuration. The loops will generally unfault to form perfect loops when the number of vacancies reaches about 40 [12]. In fcc Cu, the most stable configurations of a vacancy cluster are the stacking fault tetrahedron (SFT) and faulted clusters on {111} planes that form Frank loops with Burgers vector 1/3111. Binding energies of the various vacancy configurations in α -Fe and Cu are shown in Fig. 7.46a,b. Note that the binding energy of vacancies in the cluster is much less than that for interstitials shown in Fig. 7.43a,b. The binding energy per defect for a four-defect cluster is less than 0.4 eV for vacancies, but is about 1.2 eV for interstitials. Observation by transmission electron microscopy [16] reveals that vacancy dislocation loops and SFT a few nanometers in size are formed by cascades in many metals (Fig. 7.47).

304

7 Dislocation Microstructure Fig. 7.47. Transmission electron micrograph of (a) defect clusters in gold irradiated to 1.1 ×1022 n/m2 at 200 ◦C and (b) stacking fault tetrahedra in silver irradiated to 4.4 ×1021 n/m2 at 400 ◦C (after [16])

7.3.3 Cluster Mobility Clustered SIAs formed in cascades exhibit high mobility and can migrate over atomic scale distances during the lifetime of the cascade (∼ 10 ps). However, not all clusters are glissile. Besides stable, faulted Frank loops, SIAs may form metastable arrangement of SIAs that do not reorganize into a stable, glissile form by the end of the thermal spike. They are significant because they do not migrate away from the cascade, they may act as nucleation sites for the growth of extended defects. Figure 7.41 indicates that the fraction of SIA clusters in a metastable sessile configuration by the end of the thermal spike phase is between 30 and 50% at 100 K and somewhat less at 600 K. The form of these clusters varies with crystal structure. In hcp metals, small sessile clusters form a triangular arrangement of closely-packed atoms on the basal plane. In α -iron, three SIAs can form a triangle that is parallel to but displaced from the {111} plane. If clusters form as faulted dislocation loops, such as b = 1/3111 in fcc, 1/2110 in bcc and 1/20001 in hcp, then they are intrinsically sessile and cannot exhibit glide. The ability to move arises from the clustered crowdion form of these extended defects. They have a form best described as small perfect interstitial dislocation loops with Burgers vector b = 1/2110 in ¯ in hcp. Table 7.1 summarizes the fcc, 1/2111 and 100 in bcc and 1/31120 Burgers vectors of the glissile and sessile dislocation loops formed by vacancy and interstitial clusters. Mobile clusters can interact with other clusters or with impurity atoms such as helium. The behavior of small interstitial clusters in the presence of impurity helium atoms and vacancies is illustrated in Movies 7.1–7.3. In Movie 7.1 a SIA (green spheres) in bcc iron interacts with two substitutional He (light blue spheres) atoms and the interaction leads to recombination and ejection of the He into in an interstitial position from which it migrates and traps the other He substitutional atom. Movie 7.2 shows the interaction between a 6-SIA cluster and three substitutional He atoms. In this case, recombination and He ejection occurs with two of the three He atoms resulting in a cluster consisting of 4-SIA and one interstitial He atom, and

7.3 Defect Clusters

305

Table 7.1. Summary of Burgers vectors of glissile and sessile loops in fcc, bcc and hcp lattices (after [10]) Crystal structure

Burgers vector

Cluster mobility

fcc

b = 1/2110 b = 1/3111 SFT (vacancy) b = 1/2111, 100 b = 1/2110 ¯ b = 1/31120 ¯ b = 1/21010, 1/20001

Glissile Sessile Sessile Glissile Sessile Glissile Sessile

bcc hcp

a cluster consisting of one interstitial He and one substituional He. Movie 7.3 shows the interaction between a 6-SIA cluster and a 4-He/6-vacancy cluster. Vacancies are denoted by the red spheres. The interaction causes the recombination and rejection of He resulting in a 4-He/1-SIA cluster. The majority of SIA clusters are glissile. Di- and tri-interstitial clusters in both α -iron and copper undergo one-dimensional glide along the crowdion direction [12]. In these small clusters, the crowdion can rotate such that glide occurs in an equivalent direction. This rotation results in essentially three-dimensional motion. The rotation frequency is lower for tri-interstitials and increases with temperature for both defects. Larger clusters are essentially perfect dislocation loops with a Burgers vector along the crowdion axis, so that their movement can be considered as thermally-assisted glide in one-dimension. Figure 7.48 shows 19 and 91interstitial clusters in α -iron. Both loops extend over six (220) planes as shown in the figures at the right of each cluster. The motion of these clusters is one-dimensional and along 111. A feature of cluster motion is that the effective correlation factor is greater than unity, i.e., a cluster that has moved one step has a high probability of making the next step in the same direction. Movie 7.4 is an MD simulation of a 19-SIA cluster in bcc iron at 287 ◦C. The cluster exhibits one-dimensional motion in the direction of the Burgers vector. The activation energy for cluster motion is between 0.022 and 0.026 eV in α iron and between 0.024 and 0.030 eV in copper [12]. The activation energy is weakly dependent on the size of the cluster, allowing the cluster jump frequency to be expressed as:

νn = ν0 n−S exp(− Em /kT ) ,

(7.56)

where Em is the average effective activation energy, ν0 is the size-independent, pre-exponential factor, and the term n−S is the cluster size dependence, where a value of ∼ 0.65 for s describes the cluster size dependence of the pre-exponential factor for both α -iron and copper. Figure 7.49 shows the total pre-exponential factor as a function of cluster size. This dependence is likely due to enhanced focusing of the crowdion configuration for SIAs in a cluster, which results in increased probability of successive jumps.

306

7 Dislocation Microstructure

¯ and (b) [001] projections. Filled and open Fig. 7.48. A 19 and 91-interstitial cluster in (a) [111] circles represent the centers of mass of 111 crowdions and split dumbbells, respectively. (c) Additional (220) lattice planes occupied by the clusters (after [17])

Vacancy clusters that form perfect dislocation loops are also intrinsically glissile. MD simulation shows that the mobility of perfect vacancy loops with b = 1/2110 and 1/2111 in Cu and α -iron respectively, is only slightly lower than that of a cluster of the same number of interstitial crowdions [12]. The result is shown in Fig. 7.50 for a 37-defect cluster. As long as they are in the form of perfect loops, they are mobile. Vacancy clusters that do not collapse to a dislocation structure or that form a Frank loop or SFT are immobile.

7.4 Extended Defects As described in the previous sections, vacancies and interstitials can cluster to form other types of defects that will be important in defining the effect of irradiation on both physical and mechanical properties of the solid. In principle a cluster of point defects could be one-dimensional (a line), two-dimensional (a disc), or threedimensional (a void). Vacancies and interstitials that cluster in numbers greater than those discussed earlier will agglomerate into specific configurations in the crystal lattice. In particular they will take up the minimum energy configuration, which in

7.4 Extended Defects

307

Fig. 7.49. Size dependence of the pre-exponential factor in Eq. (7.56) in (a) α -Fe and (b) Cu (after [12])

Fig. 7.50. Jump frequency vs. reciprocal temperature for vacancy loops (squares and diamonds) and SIA loops (circles) in Fe at 375 ◦C (after [12])

308

7 Dislocation Microstructure

three dimensions is a void, and in two dimensions is a loop or platelet with a thickness of magnitude equal to one Burgers vector and lying between adjacent closepacked planes. It may be envisioned that following the radiation damage event, the core of the displacement spike collapses (or the vacancies condense) onto the {111} plane, forming a vacancy disc. The energy of the disc can be written as: Ed = 2π rd2 γ ,

(7.57)

where rd is the disc radius and γ is the surface energy of the metal. For a small number of vacancies, the aggregate form with the least energy is the spherical void. The energy of the spherical void of radius rV is: 2 EV = 4π rV γ.

(7.58)

If Ω is the atomic volume then the number of vacancies in the void is: nV =

3 4 π rV . 3 Ω

(7.59)

The energy of the void written in terms of the number of vacancies is: ES = 4 π

3nvΩ 4π

2/3

√ γ = (6nv Ω π )2/3 γ .

(7.60)

For a large number of vacancies, the planar loop is a more stable configuration and this will be discussed shortly. Another possible configuration of a cluster of vacancies is the stacking fault tetrahedron as described in Sect. 7.2. The energy of the stacking fault tetrahedron, or SFT, is given by [4, 18, 19]:

√ μ Lb2 4L (7.61) ESFT = ln + 1.017 + 0.97ν + 3L2 γSFE , 6π (1 − ν ) a where ν is Poisson’s ratio, a is the lattice parameter, γSFE is the energy of the stacking fault and L is the length of the edge of the tetrahedron and L = a(n/3)1/2. A similar process involving interstitial condensation may occur around the edges of the depleted zone where high interstitial concentrations may exist. The condensation of interstitials onto a close-packed plane produces an extra layer of atoms and two breaks in the stacking sequence, as described in Sect. 7.2 For a disc of radius rL , the energy of a faulted loop (vacancy or interstitial) is: EL = 2π rLΓ + π rL2 γSFE ,

(7.62)

where the first term is the energy of the dislocation line and the second term is the energy associated with the stacking fault, and Γ is the energy per unit length of dislocation line. In the fcc lattice, faulted loops lie on the {111} planes, which have

7.4 Extended Defects

309

√ √ an atom density of 4/ 3a2 , or an area per atom of 3a2 /4. So the radius of a loop consisting of n vacancies (or interstitials) is: √ 1/2 3a2 n . rL = 4π

(7.63)

Approximating Γ with μ b2 , Eq. (7.32b) where μ is the shear modulus and b is the Burgers vector, Eq. (7.62) becomes: √ EL = 2 π μ b

2

3a2 n 4π

1/2

√ 3a2 n +π γSFE . 4π

(7.64)

More precise expressions for the energy of faulted and perfect loops are given in [4, 6, 18, 19, 20] and from [20], the energy of the faulted Frank loop is:

2 1 4rL μ b2 rL ln − 2 + π rL2 γSFE . (7.65) EF = 3 (1 − ν ) rc The energy of a perfect loop [16] is:

4rL 1 2−ν 2 1 + μ b2 rL ln −2 , EP = 3 (1 − ν ) 3 2(1 − ν ) rc

(7.66)

where rc is the dislocation core radius. Equations (7.65) and (7.66) refer to both interstitial and vacancy loops and from these equations, the difference in energy between a perfect loop and a Frank loop is:

2−ν 1 4rL 2 2 ΔE = π rL γSFE − μ b rL ln −2 . (7.67) 3 2(1 − ν ) rc Therefore, unfaulting is favorable if:

2−ν μ b2 4rL γSFE > −2 . ln 3π rL 2(1 − ν ) rc

(7.68)

Equations for a disc, void, perfect loop, faulted loop and SFT are plotted in Fig. 7.51a,b for 316 stainless steel and zirconium respectively. The values of the materials parameters are provided in the caption. Note that in general, faulted defects are more stable in zirconium than in stainless steel and voids are more stable in stainless steel than in zirconium. In stainless steel, voids are stable to relatively large sizes and the energy of the faulted loop remains below that of the perfect loop to large defect sizes. In zirconium, faulted loops and SFTs are more stable than voids. The high susceptibility to void swelling in stainless steel and the absence of voids in zirconium are in qualitative agreement with the formation energies for these extended defects according to Fig. 7.51.

310

7 Dislocation Microstructure

Fig. 7.51. Formation energy for various vacancy cluster defects in (a) 316 stainless steel, and (b) zirconium as a function of the log of the number of vacancies in the cluster. Material parameters for stainless steel are γSFE = 35 mJ/m2 , γ = 1.75 J/m2 , μ = 82 GPa. Material parameters for zirconium are γSFE = 102 mJ/m2 , γ = 1.40 J/m2 , μ = 33 GPa

7.5 Effective Defect Production

311

Since we have just shown that the void is a stable configuration only for small numbers of vacancies, how then can we observe large voids with the number of vacancies exceeding several orders of magnitude? It is well-established that for most metals, irradiation at low temperatures (< 0.2T /Tm ) results in aggregation of vacancies and interstitials to form clusters that are bound by dislocations, i.e., loops and stacking fault tetrahedra (in metals with low SFE). At higher temperatures, vacancies can also aggregate to form voids. Voids appear in a band of temperatures ranging from about 1/3 < T /Tm < 1/2 where insoluble gases such as helium have a strong effect on stabilizing voids. At temperatures less than 1/3T /Tm , vacancies are not mobile enough to reach the voids before annihilation with migrating interstitials. Also, loops formed by vacancy collapse of cascades are stable against thermal dissociation at low temperatures and hence, reduce the number of vacancies available for void growth. At very high temperature, the thermal equilibrium vacancy concentration becomes comparable with the radiation-induced vacancy concentration and voids tend to shrink by vacancy emission. The subject of void and bubble nucleation and growth will be discussed in more detail in Chap. 8.

7.5 Effective Defect Production With a better understanding of the importance of defect clusters, we can expand and refine our description of defect production. Microstructure evolution is ultimately controlled by the migrating defect fractions of vacancies and interstitials, MDFv,i . The most straightforward component of the MDF is the isolated point defect fraction, IDFv,i (discussed in Chap. 3), which is produced directly in the displacement cascade. A second component is the mobile cluster fraction, MCFi,v (discussed in Sect. 7.3.3) and is composed of mobile interstitial defect clusters and mobile vacancy clusters. The third component is defects released from clusters by evaporation, EDFv,i , and is most important for vacancies, and interstitials at very high temperatures. Taken together, these three sources of isolated defects comprise the migrating defect fraction, MDFv,i . Zinkle and Singh [21] constructed a flow chart to show the evolution of the various defect forms (Fig. 7.52), which is an expansion of the more simplistic case shown in Fig. 3.16 by inclusion of the processes in dashed boxes. Zinkle and Singh summarized experiments from which values for MDFv,i could be determined, and found that in general, 3% < MDFi < 10%, and 1% < MDFv < 10% where the percentages refer to the calculated NRT production rate. While there is considerable uncertainly regarding the quantitative values deduced from experiments, the range can be used to bound the expected available defect fraction. The significance of these processes is that they are not often addressed in traditional rate theory models of microstructure evolution. To create an accurate physical model of defect production and accumulation under cascade damage conditions, the following must be included:

312

7 Dislocation Microstructure

Fig. 7.52. Flow chart giving the contributions to the migrating defect fraction from isolated defects, mobile defect clusters and evaporating defects (after [19])

1. The production of a large fraction of defects heterogeneously in the form of vacancy and interstitial clusters with the remainder as isolated vacancies and interstitials 2. The bias for absorption of mobile interstitial clusters and freely migrating interstitials at sinks 3. The fractions of interstitials and vacancies in clustered or isolated forms that are not necessarily equal, which is equivalent to an asymmetric production of freely migrating fractions of vacancies and interstitials

7.6 Nucleation and Growth of Dislocation Loops

313

4. Vacancy evaporation from clusters formed during the cascade quench that results in a temperature-dependent contribution to the fraction of freely migrating vacancies As will be shown in subsequent sections and in the discussion of void formation and growth in Chap. 8, intracascade clustering and the thermal stability of interstitial and vacancy clusters cause an asymmetry in the supply of migrating vacancies and interstitials, termed the production bias and this bias represents a strong driving force for loop and void nucleation and growth.

7.6 Nucleation and Growth of Dislocation Loops Dislocation loops resulting from vacancy and interstitial condensation are created from clusters of the respective defects, and either shrink or grow depending on the flux of defects reaching the embryo. Once they have reached a critical size, the loops become stable and grow until they unfault by interaction with other loops or with the network dislocation density. The following sections describe the processes of loop nucleation, growth and unfaulting that determine the dislocation microstructure of a metal under irradiation. 7.6.1 Loop Nucleation Various attempts have been made to determine the nucleation rate of dislocation loops and voids. We will follow a treatment that is based on steady sate concentrations of vacancies and interstitials and assumes dilute solution thermodynamics, as develop by Russell et al. [22]. In this treatment, the effects of cascades are ignored. We will then introduce clustering theory and show how it can be applied to the loop nucleation problem to account for the formation of defect clusters in addition to point defects. We begin by expressing the nucleation rate of a defect cluster of size n as the flux of clusters between adjacent size classes in a phase space of cluster size. Considering only one type of defect (vacancies, for example), the flux between any two adjacent size classes can be written as: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) ,

(7.69)

Fig. 7.53. Illustration of the capture and emission processes governing the flux of clusters between adjacent size classes in a phase space of cluster size

314

7 Dislocation Microstructure

where ρ (n) and ρ (n + 1) are the number of n-mers (loops containing n vacancies) and (n + 1)-mers per unit volume. βv (n) is the rate of vacancy capture by a n-mer, and αv (n + 1)is the rate of vacancy loss by a (n + 1)-mer. The first term in Eq. (7.69) represents an addition to the n + 1 size class by capture of a vacancy by a void n-mer size class. The second term is a loss from the (n + 1)-mer size class by emission of a vacancy. Figure 7.53 shows the various processes described by Eq. (7.69) in phase space. At steady state, Jn = 0 and Eq. (7.69) becomes:

αv (n + 1) = βv (n)

ρ 0 (n)

ρ 0 (n + 1)

,

(7.70)

where ρ 0 (n) is the equilibrium concentration of n-mer vacancy loops. Substituting for αv (n + 1) from Eq. (7.69) into the expression for the nucleation rate, Eq. (7.70) yields:

ρ 0 (n) Jn = βv (n) ρ (n) − ρ (n + 1) 0 ρ (n + 1) (7.71)

ρ (n + 1) ρ (n) 0 − = −βv (n)ρ (n) 0 , ρ (n + 1) ρ 0 (n) 0 and the term in brackets is just the derivative of the ratio ρ (n)/ρ (n), or 0 ∂ ρ (n)/ρ (n) . The nucleation rate then becomes: ∂n ∂ ρ (n)/ρ 0(n) 0 Jn = −βv (n)ρ (n) , (7.72) ∂n where

ρ 0 (n) = N0 exp(−ΔG0n /kT ) ,

(7.73) per unit volume, and ΔG0n

is the free energy and N0 is the number of nucleation sites of forming the n-mer vacancy loop. The steady state nucleation rate of vacancy loops (consisting of k vacancies) can also be described as the product of the loop concentration, the jump frequency of the vacancy to the loop and the jump distance, and is given by: Jk = ρk0 βk Z ,

(7.74)

where ρk0 and βk are the values of ρ 0 (n) and βv (n) at the critical size, k, and Z is the Zeldovich factor that depends on the curvature of ΔG0n near the maximum, at the critical size. If ΔG0n is approximated by a parabola in this region (lower curve in Fig. 7.54), then:

Z= −

1 ∂ 2 ΔG0n 2π kT ∂ n2

1/2 ,

(7.75)

nk

where the derivative is evaluated at the critical loop size, nk . Its value is the width of ΔG0k at kT units below the maximum and is on the order of 0.05.

7.6 Nucleation and Growth of Dislocation Loops

315

Fig. 7.54. Schematic nucleation curves showing the various parameters which are important in cluster nucleation. ΔG0k is the activation barrier to nucleation if interstitials are not present, while ΔGk is the same quantity if interstitials are present during the vacancy cluster nucleation process (after [22]) Fig. 7.55. Illustration of the capture and emission processes governing the flux of clusters between adjacent size classes in a phase space of cluster size and including the effect of interstitial capture

Consider now the presence of interstitials in the vacancy loop nucleation formulation. The flux between any two size classes, say n and n + 1, now becomes: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) − βi(n + 1)ρ (n + 1) ,

(7.76)

where all terms are as previously defined, and βv (n + 1) is the rate of interstitial capture by a (n + 1)-mer. Interstitial emission is of low probability and is neglected. Figure 7.55 shows the various processes described by Eq. (7.76) in phase space. The rate of vacancy emission from a vacancy loop will be governed by temperature, size and lattice energetics. Since the defect fractions are as high as 10−4, a cluster has a defect in its immediate vicinity only this small fraction of time. The emission probability should be affected only slightly during this time interval and not at all otherwise. Therefore we conclude that αv is a value characteristic of a system without interstitials. Setting J = 0 in Eq. (7.76) is equivalent to equilibrating the size classes since there is no net flux between size classes. If we neglect interstitials, then from Eq. (7.76) we can write:

αv (n + 1) =

βv (n)ρ 0 (n) . ρ 0 (n + 1)

(7.77)

316

7 Dislocation Microstructure

Combining Eqs. (7.76) and (7.77) gives:

0 ρ (n) βi (n + 1) + Jn = βv (n) ρ (n) − ρ (n + 1) 0 . ρ (n + 1) βv (n) Since ρ 0 (n) = N0 exp(−ΔG0n /kT ), then we note that: 0 ρ 0 (n) δ Gn = exp , ρ 0 (n + 1) kT

(7.78)

(7.79)

where δ G0n ≡ ΔG0n+1 − ΔG0n . The term δ G0n is the difference between the free energies of creating loops of j + 1 and j vacancies from single vacancies at the prevailing supersaturation. We now define new functions of n, ρ (n) and δ Gn such that by analogy with Eq. (7.79):

ρ (n)

ρ (n + 1)

=

ρ 0 (n)

ρ 0 (n + 1)

+

βi (n + 1) = exp(δ Gn /kT ) , βi (n)

(7.80)

where

δ Gn = ΔGn+1 − ΔGn ,

(7.81)

βi (n + 1) in Eq. (7.81). βi (n) Using the expression in Eq. (7.81), we can re-write the equation for Jn in terms of ρ (n) by substituting Eqs. (7.80) into (7.78) to give: ρ (n + 1) ρ (n) Jn = βv (n) ρ (n) − ρ (n + 1) . (7.82) ρ (n + 1)

and ΔGn is not generally a free energy because of the term

Re-arranging Eq. (7.82) gives: Jn = −βv (n)ρ (n)

ρ (n + 1) ρ (n) − , ρ (n + 1) ρ (n)

and noting that:

ρ (n + 1) ρ (n) ρ (n) − ∂ ρ (n + 1) ρ (n) ρ (n) = , Δn ∂n

(7.83)

(7.84)

gives: Jn = −βv (n)ρ (n)

∂ [ρ (n)/ρ (n)] , ∂n

(7.85)

which is the basic flux equation. Re-arranging Eq. (7.85) by taking the natural log of both sides and summing from j = 0 to n − 1 gives: n−1 n−1 δ G0j ρ ( j) βi ( j + 1) , (7.86) ∑ ln ρ ( j + 1) = ∑ − ln βv ( j) + exp kT j=0 j=0

7.6 Nucleation and Growth of Dislocation Loops

and

ρ (n) ln ρ (0)

=

n−1

∑

j=0

317

δ G0j βi ( j + 1) − ln + exp . βv ( j) kT

(7.87)

We can identify two boundary conditions. The first is the quantity ρ (0), which may be evaluated by noting that as βi (n)/βv (n) → 0, ρ (0) = ρ 0 (0) and that ρ 0 (0) → N0 , is simply the number of nucleation sites per unit volume. Since N0 (and hence ρ (0)) is independent of void concentration, we can write: n−1 δ G0j −ΔGn ρ (n) βi ( j + 1) + exp , (7.88) = − ln ln = ∑ ρ (0) βv ( j) kT kT j=0 and ΔGn

δ G0j βi ( j + 1) + exp . = kT ∑ ln βv ( j) kT j=0 n−1

(7.89)

Since as βi (n)/βv (n) → 0, ρ (0) → ρ 0 (0) and ρ 0 (0) is just N0 , the number of nucleation sites per unit volume, we have then: −ΔGn ρ (n) = N0 exp , (7.90) kT and

ΔG0n = activation barrier without interstitials ΔGn = activation barrier with interstitials. The upper curve in Fig. 7.54 shows ΔGn as functions of n. Note that ΔGn is larger than ΔG0k , and requires a larger loop size due to the hindering effect of interstitials on the loop nucleation process. The maxima in the two curves occur at nk , ΔG0k and nk , ΔGk . Now, the steady state loop nucleation rate may be calculated from the expression for Jn in Eq. (7.85): Jk = Z βk ρk ,

(7.91)

which is the rate at which loops escape over the potential barrier of height ΔGk in units of loops/cm3 s. The term βk , is the rate of single vacancy impingement on a loop of size nk . The term Z is:

1/2 1 ∂ 2 ΔGn Z = − . (7.92) 2π kT ∂ n2 n k

The subscript indicates that the second derivative is to be evaluated at n = nk . As with Z in Eq. (7.75), its value is the width of Δ Gk at kT units below the maximum and is of the order of 0.05. The second derivative is found from Eq. (7.69) to be:

1 ∂ 2 ΔG0n 1 ∂ ΔG0 1 ∂ 2 ΔGn = , (7.93) exp kT ∂ n2 kT ∂ n2 kT ∂ n n n k

k

318

7 Dislocation Microstructure

giving:

ρk = N0 exp −ΔGk /kT ,

(7.94)

where ΔGk is determined by evaluating Eq. (7.89) at nk . The steady state nucleation rate will not be established immediately after a sudden change in supersaturation or temperature, but will lag by a characteristic time, τ , known as the incubation time and is given by [22]:

τ = 2(βk Z 2 )−1 .

(7.95)

Equations (7.89) and (7.94) also apply for interstitial loop nucleation except that Z , βk and ρk are for interstitial loops rather than for vacancy loops, and ΔGn for interstitial loops is: n−1 δ G0j βv ( j + 1) ΔGn = kT ∑ ln + exp , (7.96) βi ( j) kT j=0 where δ G0j is now the difference between the free energies of forming dislocation loops of j + 1 and of j interstitials (in the absence of vacancies), βk is the gross rate of interstitial capture by the loop of critical size and 1/Z is the width of ΔGn (for interstitials) a distance kT below the maximum at ΔGk , and the net number of interstitials in the critical nucleus is denoted by nk . The critical loop size, nk occurs at the maximum of ΔGn and is determined by solving ∂ ΔGn /∂ n = 0 for nk . More recent treatments of the nucleation rate call for setting the all the fluxes in Eq. (7.69) equal to the steady state flux, Jss , leading to a family of equations [23]: J1 = βv (1)ρ (1) − α (2)ρ (2) = Jss

(7.97)

J2 = βv (2)ρ (2) − α (3)ρ (3) = Jss J3 = βv (3)ρ (3) − α (4)ρ (4) = Jss .. . Jn−1 = βv (n − 1)ρ (n − 1) − α (n)ρ (n)

(7.98) (7.99)

(7.100)

k where n = nmax v . Letting the ratio of shrinkage to growth, αk /βv = rk for all k ≤ 2, and letting r1 = 1, the system of equations can be solved by multiplying the equations for Jk by the product of all the rk with k ≤ i. That is, Eq. (7.98) is multiplied by r2 , Eq. (7.99) is multiplied by both r2 and r3 , and so on. If the resulting set of equations is summed, all the rk are eliminated except r1 and rn to yield: n−1

βv (1)ρ (1) − α (n)ρ (n) ∏ r j J1 = Jss =

j=2

n−1 k

.

(7.101)

1 + ∑ ∏ rj k=2 j=2

The product term in the numerator is eliminated by noting that (1) for a nucleation problem, the concentration of the monodefect, ρ (1) will be much greater than ρ (n),

7.6 Nucleation and Growth of Dislocation Loops

319

and (2) the ratio of the shrinkage to growth terms r j is less than unity for n > n∗v . Therefore, Eq. (7.101) becomes:

n−1 k

Jss = βv (1)ρ (1) 1 + ∑

∏ rj

−1 .

(7.102)

k=2 j=2

The advantage of this method to compute Jss is the elimination of the Zeldovich factor and the approximations that must be made to compute it. Russell [22] determined that based on vacancy and interstitial parameters and their likely supersaturations in a solid under irradiation, that interstitial loop nucleation is easier than vacancy loop nucleation because interstitial loop nucleation is much less sensitive to vacancy involvement than is vacancy loop nucleation to interstitial involvement. The primary reason is that Si is expected to be several orders of magnitude greater than Sv during irradiation because of the very low equilibrium concentration of interstitials. Nevertheless, nucleation by this mechanism has been found to be difficult for both vacancy and interstitial loops, in contrast to the observation of stable loop growth after fairly low doses. 7.6.2 Clustering Theory The nucleation of loops is essentially a clustering process in which enough of one type of defect needs to cluster, in the presence of the other type of defect, to result in a critical size embryo that will survive and grow. The cluster will shrink or grow depending on the net condensation rate of defects on clusters. Generalizing the description of cluster behavior in phase space given in the last section, and taking a vacancy loop as an example, vacancy clusters, ν j consisting of j vacancies will shrink or grow according to: j ∞ dν j = K0 j − ∑ [βvn ( j) + βin ( j)]ν j − ∑ αvn ( j)ν j dt n−1 n=1 j−1

∞

n=1 ∞

n=1

+ ∑ βvn ( j − n)ν j−n + ∑ βin ( j − n)ν j+n

(7.103)

+ ∑ αvn ( j + n)ν j+n + additional loss terms n=1

where βvn and βin are the capture rates of migrating defect clusters νn or in by a cluster of size ν j , and αvn is the corresponding emission or thermal dissolution rate. The first term on the RHS is the direct production of clusters of size j. The second term is the loss of clusters from size class j due to absorption of a vacancy or an interstitial cluster of size n, where 1 n ∞. The third term is the loss of clusters from size class j due to emission of vacancy clusters of size n. The fourth and fifth terms are the addition of clusters to size class j due to absorption of vacancy clusters by smaller size classes, and the absorption of interstitial

320

7 Dislocation Microstructure

clusters by larger size classes. The sixth term is the addition of clusters to the size class j by loss of vacancy clusters from larger size classes and the “additional loss terms” allow for other mechanisms of contributing to the number of clusters in size class j. Equation (7.103) can be solved numerically without further simplification. But for large clusters and long irradiation times, the number of equations required would be extremely large. A major simplification is to require clusters to grow or shrink by only the addition or loss of single point defects, resulting in: dν j (t) = K0 j + β ( j − 1, j)ν j−1(t) + α ( j + 1, j)ν j+1 (t) dt − [β ( j, j + 1) + α ( j, j − 1)]ν j (t) , j ≥ 2 .

(7.104)

If it is assumed that j is a continuous variable and a Taylor series expansion is used in Eq. (7.104) to relate all functions to their values at size j, the simplified description is a continuum diffusional approximation in size space, known as a Fokker–Planck equation: * ∂ ν j (t) ∂ ) = K0 j (t) − ν j (t) [β ( j, j + 1) − α ( j, j − 1)] ∂t ∂j * 1 ∂2 ) ν j (t)[β ( j, j − 1) + α ( j, j + 1)] , + 2 2∂j

(7.105)

which is further simplified to:

∂ ν j (t) ∂ ∂2 = K0 j (t) − Fv j ν j (t) + 2 Dv j ν j (t) ∂t ∂j ∂j ∂ ∂ = K0 j (t) − Fv j ν j (t) − Dv j ν j (t) . ∂j ∂j

(7.106)

The first term on the RHS of Eq. (7.106) is the direct production rate of clusters of size j. The second term is the drift in size space driven by the excess condensation of one point defect type over another: Fv j = (zv DvCv − zi DiCi )

(7.107)

The drift term is responsible for the shift of the cluster size distribution to larger sizes. The drift term ensures that a large cluster will inevitably grow in a radiation field, but due to the evolving microstructure, the drift contribution is not constant with dose. Cluster evolution is also very sensitive to the ratio of the concentration of vacancies and interstitials, as Fv contains the difference in their contribution and can change sign. The result is that the sign of Fv depends on the overall microstructure. The third term is the diffusion in size space and Dv j is the irradiation-enhanced diffusion coefficient given by: Dv j = 1/2(zv DvCv + zi DiCi ) .

(7.108)

7.6 Nucleation and Growth of Dislocation Loops

321

Fig. 7.56. Development of the interstitial loop size distribution with dose in 316 stainless steel irradiated at a dose rate of 10−6 dpa/s and a temperature of 550 ◦C with ρd = 1013 m−2 (after [25])

The diffusion term causes the cluster size distribution to broaden with dose. The diffusion term accounts for the fact that two different clusters introduced at the same time at the same size may differ in size at a later time due to random encounters with point defects. Algorithms for the approximate solution of Eq. (7.106) are discussed by Golubov et al. [24]. The features of the Fokker–Planck equation are illustrated in Fig. 7.56 for the development of the interstitial loop size distribution for 316 stainless steel with initial dislocation density of 1013 m−2 , irradiated at 550 ◦C at a dose rate of 10−6 dpa/s. Note that with increasing dose, the mean loop size increases (drift term in Eq. (7.106)) and the size distribution broadens (diffusion term in Eq. (7.106)). As small clusters grow and their geometry changes, so does the capture efficiency for freely migrating defects. For very large cluster sizes, the Fokker– Planck equation is too simple as the defect production and cluster growth depend on the microstructure. The effect of the damage microstructure in the evolution of defect clusters must be accounted for in order to accurately predict their behavior. 7.6.3 Production Bias-Driven Cluster Nucleation As discussed both in Chap. 3 and in the Sects. 7.3 and 7.4 of this chapter, a significant fraction of point defects produced under cascade damage irradiation are in the form of mobile and immobile vacancy and interstitial clusters such that freely migrating interstitials and vacancies are produced in unequal numbers. This has led to the concept of production bias as a major driving force for microstructure evolution under cascade-producing irradiation, and is based on the premise that defects

322

7 Dislocation Microstructure

in clusters do not behave as freely migrating defects. In fact, as we have seen, interstitial clusters can be mobile and exhibit 1D and 3D glide. In some cases, the clusters remain mobile to very large size, though generally, there is a tendency toward the sessile state with increasing size. This picture of defect formation describes an asymmetry, or bias, in the production of freely migrating point defects under cascade damage conditions due to two sources: (1) the difference in the proportion of vacancies and interstitials that agglomerate into primary clusters, and (2) the difference in the thermal stability and mobility of the vacancy and interstitial clusters. Under cascade conditions, in addition to the probabilistic nature of point defect jumps, the random production, in space and time, of clusters also introduces fluctuations in the point defect fluxes to the sinks. The production bias model (PBM) is a framework for considering this added complication in the evolution of the microstructure under irradiation. Semenov and Woo [26] utilized the Fokker–Planck treatment of cluster dynamics presented in the last section to produce a revised description of the loop nucleation rate that incorporates the effect of small interstitial cluster generation in the collision cascade produced randomly in time and space. They considered that small, immobile interstitial clusters are continuously generated in collision cascades, and that these clusters can be treated as small dislocation loops. The probability density, P of an interstitial cluster with a size of n0 interstitials at a time t0 , to grow to a size of n interstitials at time t is: ∂ Pi (n,t) ∂ ∂ =− (7.109) Fi (n) − Di (n) Pi , ∂t ∂n ∂n where the diffusion term, Di (n) describes the spreading of the size distribution of interstitial loops in time due to random fluctuations in the isolated and clustered point defect fluxes and is given by: Di (n) = Dsi (n) + Dcl i (n) ,

(7.110)

with superscripts s and cl denoting single defects and clusters, respectively, and: π n 1/2 (zv DvCv + zi DiCi ) , (7.111) Dsi (n) = Ω b + 2, + 2 , N Nd K0 n 2 Ndv zv Dcl + z2i di2 . (7.112) i = 4b kv Nd2 ki Nd In the preceding, K0 is the effective point defect generation rate (cluster + 2and , free), Nd is the average number of point defects generated per cascade and Ndv,i is the 2 average of the square of the quantity, kv,i are the total sink strengths for vacancies and interstitials, zvi are the bias factors for vacancies and interstitials, and b is the magnitude of the Burgers vector. The drift term has two components, Fis (n), and Fic (n). Fis (n) =

2π ri (n) (zi DiCi − zv DvCv ) , Ω

(7.113)

7.6 Nucleation and Growth of Dislocation Loops

323

is the term that drives the growth rate of loops and the loop radius:ri = (ni Ω /π b)1/2 and Ci,v and Di,v are the average concentration and diffusion coefficient of the defects. 2π ri (n) n Fic (n) = x fil (x,t)W (x, n) dx , (7.114) Ω n0 is the rate of change in the loop size due to the absorption of smaller interstitial loops by coalescence. The function fil (n,t) is the distribution of interstitial loops which is related to the total loop number density, Nil (t) by: Nil (t) =

nmax nmin

fil (n,t) dn ,

(7.115)

and nmin is the size of the interstitial clusters at which they become mobile and nmax is the size at which they join the network. The term W (n , n) describes the coalescence between loops of sizes n and n (n < n): 1/2 2 (n)λd2 4ri (n ) 2 D (n) + D (n) + , (7.116) W (n , n) = λd 4 where λd is the mean free path between two consecutive coalescing events, is the climb velocity and D (n) is the climb diffusion coefficient due to the fluctuating point defect fluxes and is given as: D (n) = Ds (n) + Dcl (n) ,

(7.117)

with:

Ω (zv DvCv − zi DiCi ) , 4π b2ri (n) + , + 2 , 2 Nd K0 Ω cl 2 Ndv 2 Ndi D = + zi zv . 16π b2 kv Nd2 ki Nd2 Ds (n) =

(7.118) (7.119)

Subject to the boundary conditions: Pi (nmin ,t)|n0 ,t0 = Pi (nm ,t)|n0 ,t0 = 0 , the solution to Eq. (7.109) is given by Semenov and Woo [26] to be: n0 x Fis (x ) dx dx nmin exp − nmin Di (x ) Pm = , n0 Fis (x ) ∗) x dx exp −(1 − α dx nmin nmin Di (x )

(7.120)

(7.121)

where

α∗ =

Fic (n ) (nmin < n < n∗ < nm ) . Fis (n )

(7.122)

324

7 Dislocation Microstructure

The term α ∗ is the ratio of the rate of loop size change due to cluster coalescence to that due to point defect absorption, or essentially, the relative importance of cluster coalescence compared to defect absorption. Semenov writes the integrals in the exponential functions in Eq. (7.120) as:

s Fi (x) 2 fs 1/2 ds ds 1/2 dx = ln n +1 , (7.123) n − dcl dcl dcl n Di (x) where Fis (n) Dsi (n) Dcl i (n) , d = , d = . (7.124) s cl 1/2 1/2 n n n1/2 The two limiting cases are when defect absorption is unimportant, dcl → 0, and when cluster coalescence is minimal, ds → 0. For the case dcl → 0, Eq. (7.121) becomes: fs =

exp(− fs n0 /ds ) − exp(− fs nmin /ds ) exp(− fs nm (1 − α ∗)/ds ) − exp(− fs nmin (1 − α ∗)/ds ) × exp(α ∗ fs nmin /ds ) ,

Pm = (1 − α ∗)

(7.125)

and for the case ds → 0, Eq. (7.121) becomes:

1/2 1/2 1/2 1 + 2 fsn0 /dcl exp −2 fs n0 /dcl Pm = (1 − α ∗ )2 exp 2α ∗ fs nmin /dcl

. 1/2 1/2 − 1 + 2 fsnmin /dcl exp −2 fs nmin /dcl

- 1/2 1/2 / 1 + 2(1 − α ∗) fs nmin /dcl exp −2(1 − α ∗) fs nmin /dcl

. 1/2 1/2 . − 1 + 2(1 − α ∗) fs nmin /dcl exp −2(1 − α ∗) fs nmin /dcl (7.126) The behavior of Pm as a function of the number of interstitials in the cluster is shown in Fig. 7.57. In this case, α ∗ = 0 and the solid lines are for the case where ds → 0, Eq. (7.126), and the dashed lines are for the case were dcl → 0, Eq. (7.125). The dashed line at the lower left in the figure resulted when clusters are ignored. However, when clustering is considered (solid lines) the nucleation probability increases substantially. In fact, if we define εi0 to be the fraction of interstitials produced in cascades in the form of immobile clusters, and K0 is the interstitial production rate, then εi0 K0 /n0 is the production rate of interstitial clusters in the cascade, and the nucleation rate of interstitial loops is: J =

εi0 K0 Pm . Ω n0

(7.127)

Choosing the following values; εi0 = 0.4, Pm ∼ 10−6 , Ω ∼ 10−29 m3 , n0 ∼ 8, gives ∼ 5 ×1021 loops/m3 per NRT dpa. Given that loop densities are observed to be about this value, then the incubation dose is on the order of 1 NRT dpa. However, this value for the nucleation incubation time is high as small loops are readily observed in transmission electron microscopy of irradiated materials at fractions of a dpa.

7.7 Dislocation Loop Growth

325

Fig. 7.57. Interstitial cluster nucleation probability as a function of loop size. In this figure, α ∗ = 0 and the solid lines are for the case where ds → 0, Eq. (7.126), and the dashed lines are for the case were dc → 0, Eq. (7.125). The dashed line at the lower left in the figure is result when clusters are ignored (after [26])

7.7 Dislocation Loop Growth The growth of loops can also be determined from the Fokker–Planck equations that provide the size distribution of loops of all sizes (see Fig. 7.56). Applying Eq. (7.104) to the case of interstitial loops gives an equation of the form: di j = dt K0 j + [βv ( j + 1) + αi( j + 1)]i j+1 − [βv ( j) + βi ( j) + αi ( j)]i j + βi ( j − 1)i j−1 , (7.128) where i j is the concentration of interstitial loops of size j and the term on the LHS of Eq. (7.128) is the time rate of change of the population of interstitial loops of size j. The terms βk ( j) and αk ( j) are the absorption and emission rates of defects of type k from loops of size j. The first term on the RHS of the equality is the direct production rate of clusters of size j. Practically, this term is different from zero up to the tetrahedral cluster ( j = 4). The first term in square brackets is the production of clusters of size j by the emission of an interstitial or absorption of a vacancy by clusters of size j + 1. The second term in square brackets is the loss of clusters of size j by absorption of a vacancy or an interstitial, or emission of an intertstitial. The last term is the addition of clusters of size j by capture of an interstitials by clusters

326

7 Dislocation Microstructure

of size j − 1. Solution of Eq. (7.128) results in the loop size distribution as a function of time, which describes the evolution of interstitial loops with dose or time. Pokor et al. [27] used the Fokker–Planck formalism to model the evolution of a population of loops via chemical rate theory in a homogeneous medium. In their treatment, they allowed for production of clusters in the cascade containing up to four defects, and solved a set of equations for the concentration of defect clusters consisting of two equations for individual vacancies or interstitials and 2N equations for the population of loops up to size N. The physics of the formulation is contained in the expressions for the defect capture rates, β , and emission rates, α for each defect type, k as a function of the cluster size, given as [27]:

βk ( j) = 2π r( j)zc ( j)DkCk , Dk αk ( j) = 2π r( j)zc ( j) exp(−Ebk ( j)/kT ) , Ω

(7.129) (7.130)

where r( j) is the radius of an interstitial loop of size j, Dk andCk are the diffusion coefficient and concentration of defect k, zc ( j) is the bias factor for the interstitial loop of size j and Ebk ( j) is the binding energy of for a cluster of j defects of type k. Pokor [27] gives the following expressions for zc ( j) and Ebi : b 1 zli − zi , (7.131) zc ( j) = zi + a 8π a j li /2 Ebi = Efi +

Eb2i − Efi 0.8 ( j − ( j − 1)0.8) , 20.8 − 1

(7.132)

where zi is the bias factor for a straight dislocation line for interstitials, a is the lattice parameter and b is the Burgers vector, zli and ali are parameters used to describe the evolution of the bias with cluster size [28]. For the binding energy term, Efi is the formation energy of an interstitial point defect Eq. (4.16), Eb2i is the binding energy of a two-interstitial cluster and j is the number of defects in a cluster of size j and the expression comes from molecular dynamics simulations [29, 30]. In order to account for the effect of the annihilation of the network dislocation density with dose, they assumed that the rate of change of the density was proportional to ρ 3/2, giving dρ / dt = −Kb2ρ 3/2 , and resulting in a dislocation density that decreases as 1/t 2 (see next section). The network dislocation density in irradiated metals evolves toward a saturation value with increasing dose. In stainless steel, it has been observed to reach a saturation value of ∼ 6 ×10−10 cm−2 over a temperature range that spans 400 to 600 ◦C [31]. Cluster model results of the loop density and size for three grades of stainless steel irradiated at 330 ◦C and to doses up to 40 dpa calculated using Eqs. (7.128)–(7.132) are compared against measurements in Fig. 7.58 and show relatively good agreement. Dislocation recovery plays an important role in microstructure evolution as it represents a change in sink density. Failure to account for the recovery of the initial dislocation network would lead to a faster saturation of the loop structure in the 316 alloys. The most sensitive param-

7.7 Dislocation Loop Growth

327

Fig. 7.58. Evolution of the Frank loop (a) density and (b) size for 330 ◦C irradiation to high dose according to the cluster dynamics model of Pokor et al. (after [27])

eters controlling the irradiation microstructure are the temperature, dose, materials constants and the initial network dislocation density. Simpler treatments for determining the loop size distribution can be made by neglecting the formation of defect clusters larger than the tetra-interstitial, limiting the number of size classes and simplifying the cluster description. Stoller et al. [32] described the evolution of larger loops by the equation: di j −1 (7.133) = i j−1 τ −1 j − i j τ j+1 , dt where i j is the number of loops in a given size class with radius rL , and the τ j is the lifetime of a loop of size j against growth to the next larger size class: r j+1 drL −1 τj = drL , (7.134) dt rj

328

7 Dislocation Microstructure

Fig. 7.59. (a) Comparison of calculated maximum faulted loop density and low fluence fast reactor data as a function of temperature. (b) Dose dependence of faulted loop density for irradiation of solution annealed stainless steel at 500 ◦C (after [32])

and drL Ω = [ziL (rL )DiCi − zvL(rL )Dv (Cv − CvL )] , dt b

(7.135)

where ziL and zvL are given by Eq. (5.97) and CvL = Cv0 exp(EF Ω /kT ), where EF is the energy of a faulted loop from Eq. (7.65). Figure 7.59a shows a comparison of the temperature dependence of the calculated maximum faulted loop density and

7.8 Recovery

329

low fluence fast reactor data for 316 stainless steel with initial network dislocation densities of 3 ×1015 m−2 (solid line) and 3 ×1013 m−2 (dashed line). Figure 7.59b shows the dose dependence of the loop density for solution annealed 316 irradiated at 500 ◦C. Semenov and Woo [26] accounted for the effect of production bias by writing Eq. (7.135) for the rate of change in loop size to include terms due to interstitial cluster and vacancy cluster absorption:

Ω drL = [Ji − Jv + Jve + Jicl − Jvcl ] , dt b

(7.136)

where the Js are the fluxes due to single interstitials, single vacancies, vacancy thermal emission, interstitial clusters and vacancy clusters, respectively, and τd is the lifetime of the dislocation loop. Substituting for the fluxes [32] results in: 2 kV (εi − εv ) + kd2 z¯(1 − εi) K e K0 drL = − , (7.137) dt (ρN + ρL)b k2 K0 where K0 is the defect production rate, K e is the vacancy thermal emission rate, ρn and ρL are network and loop dislocation densities, εi,v are the fraction of interstitials and vacancies, respectively, that are immobilized by intracascade clustering, 2 are the sink strengths of voids and εv = εv − K e /K0 , zd is the dislocation bias, kV,d zd k2 dislocations, k2 is the total sink strength and z¯ = 2 c 2 . The steady state interstik + zd kd tial loop growth rate for 316 stainless steel with an effective point defect production rate of 10−7 dpa/s is shown as a function of temperature in Fig. 7.60. The growth rate is in units of Burgers vector, b per dpa. Note that the loop growth rate is low at low and high temperatures and peaks at an intermediate temperature of about 500 ◦C.

7.8 Recovery Growing dislocation loops eventually encounter either network dislocations or each other. The maximum radius to which a loop can grow, Rmax , is governed by the 4π loop density, ρL as given by ρL R3max = 1. When loops interact, they coalesce 3 and contribute to the network dislocation density. Interaction between individual dislocations and loops results in loop unfaulting that also contributes to the network (discussed in Chap. 12, Sect. 12.3). As the dislocation density increases, the rate of loop interaction with the network increases and the loop radius is further limited by the network dislocation density as described by Eq. (5.82), (π R2max )ρN = 1. However, observations of irradiated microstructures confirm that the dislocation density saturates, implying that there must also be a process for removal of network dislocations limiting their buildup. The process of recovery can explain the behavior of the dislocation density with irradiation. The rate of change of the dislocation

330

7 Dislocation Microstructure

Fig. 7.60. Interstitial loop growth rate in units of Burgers vector, b per dpa as a function of temperature for a 316 stainless steel (after [33])

density in a solid under stress at high temperature is assumed to behave according to:

ρ˙ = Bρ − Aρ 2 ,

(7.138)

where ρ is the density of mobile dislocations and A and B are constants. (Note that while the rate of dislocation density change given by Eq. (7.138) is phenomenological by nature, a more accurate description of the physical process is provided by Eq. (7.133)). The first term of Eq. (7.138) is the production rate of dislocations and the second term is the annihilation rate. The loss term is assumed to occur due to mutual annihilation of pairs of dislocations of opposite sign, which implies a reaction rate that is proportional to the square of the number of dislocations present at a given time. Garner and Wolfer [34] showed that the generation rate of dislocations is proportional to b2 φ ρ 1/2 , so that Eq. (7.138) can be written as:

ρ˙ = Bρ 1/2 − Aρ 3/2 ,

(7.139)

where B ∼ b2 φ and A ∼ c , where c is the climb velocity of the dislocation (see Chap. 14). At steady state ( dρ / dt = 0), and the saturation density is ρs = B/A. The solution to Eq. (7.138) is given as: " ρ (t) 1 − e−x + ρ0 /ρs (1 + e−x ) " = , (7.140) ρs 1 + e−x + ρ0 /ρs (1 − e−x )

7.8 Recovery

331

Fig. 7.61. (a) Calculated dislocation density evolution in 316SS at 500 ◦C using Eq. (7.139), for starting densities of 7 ×1011 cm−2 and 4 ×108 cm−2 , for cold-worked and annealed conditions, respectively (after [34]). (b) Measured dislocation density in 20% cold-worked and annealed 316SS after irradiation in EBR-II at 500 ◦C (after [35])

where ρ0 is the initial dislocation density and √ √ x = A ρs t = ρs c t .

(7.141)

Using a saturation density, ρs of 6 ×1010 cm−2 , and initial dislocation densities, ρ0 of 3 ×108 cm−2 for annealed 316 SS and 7 ×1011 cm−2 for 20% CW 316 SS, the dislocation densities calculated from Eq. (7.139) are shown in Fig. 7.61a. The relationship between x in Eq. (7.140) and fluence was defined by the case where

332

7 Dislocation Microstructure

the dislocation density for annealed 316 SS reached a value of 2 ×1010 cm−2 at 2 ×1022 n/cm2. Data are plotted in Fig. 7.61b. Note how well the model results of Fig. 7.61a agree with the data. This agreement also establishes that the original dislocations are no different from those produced during the irradiation with regard to their ability to absorb point defects.

7.9 Evolution of the Interstitial Loop Microstructure The evolution of the interstitial loop population can be described in terms of its response to temperature and dose. The temperature regime that is important for LWR operation is between 270 and 340 ◦C. Higher temperatures may be reached from gamma heating in certain thick components such as PWR baffle plates. This temperature range represents a transition region between what is commonly termed as low-temperature (50 – 300 ◦C) and high-temperature (300 – 700 ◦C) behavior. Below 300 ◦C, the dislocation microstructure is characterized by a high density of “black dots” (defect clusters that are too small to resolve in the TEM, < 2 nm), network dislocations and a low density of Frank loops. A very small percentage of the small loops in stainless steels are observed to be SFT, which is much less than the 25 – 50% of clusters in nickel or copper [10]. Near 300 ◦C, the radiationinduced microstructure changes from one dominated by small dislocation loops to one containing larger faulted loops and network dislocations (Fig. 7.62). Figure 7.63 shows large dislocation loops after irradiation at high temperatures. Above

Fig. 7.62. Effect of irradiation temperature in the range 50 – 400 ◦C on the components of the dislocation density in neutron-irradiated austenitic stainless steel (after [36])

7.9 Evolution of the Interstitial Loop Microstructure

333

Fig. 7.63. Images of large Frank loops in (a) a 300 series stainless steel irradiated at 500 ◦C to a dose of 10 dpa (from [37]), and (b-e) in irradiated aluminum, copper, nickel and iron, respectively (after [16])

334

7 Dislocation Microstructure

Fig. 7.64. Effect of temperature on the Frank loop density in the intermediate temperature region, 400 – 600 ◦C, for neutron-irradiated austenitic stainless steel (after [36])

300 ◦C, the Frank loop population begins to decrease. Figure 7.64 shows the sharp decrease in faulted loop density by a factor of over 1000 between 400 and 600 ◦C in neutron-irradiated austenitic stainless steels. The loop size increases with increasing temperature that eventually leads to an increase in the loop unfaulting rate which contributes to the reduction in Frank loop population at high temperature. Loop density increases rapidly to saturation at low irradiation temperatures. Figure 7.65 shows the increase in loop density in austenitic stainless steels irradiated near 300 ◦C. Loop size is relatively insensitive to fluence below about 300 ◦C. At these low temperatures, loop sizes and densities become dynamically stable as a population when a balance is reached between new loop formation and the destruction of existing loops. With increasing temperature in the low-temperature regime, the density of fine loops decreases and the loop size increases. The dislocation microstructure evolves into one composed of Frank loops and network dislocations above about 300 ◦C. Loop density saturates at a few dpa and the density is maintained (in a dynamic sense) at higher doses. The dislocation network density increases in proportion to the faulted loop density as temperature is increased though the overall dislocation density is expected to stay fairly constant between 300 and 370 ◦C. In the higher temperature regime (400 – 600 ◦C), the population consists of a low density of Frank loops and a dislocation network. Evolution may actually occur more slowly if other microstructural processes are also occurring such as void and bubble nucleation and growth.

Nomenclature

335

Fig. 7.65. Evolution of the Frank loop density and size in various austenitic stainless steels following irradiation to doses of up to 13 dpa at a temperature near 300 ◦C (after [38])

The description of defect cluster nucleation and evolution provides a backdrop for understanding the phenomenon of void growth discussed in the next chapter. As will be shown, void formation and growth is intimately linked to the production of defect clusters and their growth into loops, as these microstructures constitute critical sinks that will govern the fate of voids.

Nomenclature a A b Cv,i 0 Cv,i x d Dv,i Dk j Dl E Eb Ef El

Lattice constant Area of slip plane Burgers vector Concentration of vacancies, interstitials Thermal equilibrium concentration of vacancies, interstitials Strength of diffusive spread for clusters by the x process Diffusion coefficient of vacancies, interstitials Diffusion term in size space of defect k and cluster size j, Eq. (7.106) Climb diffusion coefficient Energy Binding energy Formation energy Dislocation loop energy

336

Em Em Fk j

7 Dislocation Microstructure

Pi (n,t) Pm r rc rL rk s T Sv,i ui j g vn V W zv,i Z

Migration energy Effective activation energy for cluster motion Drift velocity in size space of defect k and cluster size j Eq. (7.106) Effective Frenkel pair production rate of species j Change in free energy Standard free energy Cluster of n interstitials Boltzmann’s constant Total sink strength for vacancies, interstitials Length of dislocation line segment Length of edge of stacking fault tetrahedron Nucleation current. Also flux Defect production rate Vacancy thermal emission rate Stress exponent in relation between dislocation velocity and shear stress Unit vector Critical cluster size Average number of defects generated in a single cascade Number density of interstitial loop Number of lattice sites per unit volume. Also number of nucleation sites Probability of growing an interstitial cluster to size n in time t Loop nucleation probability Defect cluster radius Dislocation core radius Loop radius Critical cluster radius Positive direction of the dislocation line Temperature. Also PKA energy Supersaturation of vacancies, interstitials Components of the displacement vector Dislocation glide velocity Cluster of n vacancies Volume Work Vacancy, interstitial bias factor Zeldovich factor Eq. (7.75)

αj βj γ γSFE δ

Emission rate of species j Absorption rate of species j Shear strain,. Also surface energy Stacking fault energy Thickness of void shell

Gj ΔG G0 in k 2 kv,i l L J K0 Ke m n nk , nk Nd Nil N0

Nomenclature

εc εi j εi0 Γ λ λd μ ν ρ (n) νs Ω ρx σ , σi j σs σsD τ τd

Strain associated with the dislocation core Components of strain Fraction of interstitials produced in cascades in the form of immobile clusters Dislocation line tension Lam´e constant Mean free path between consecutive interstitial cluster coalescing events Shear modulus Poisson’s ratio. Also jump frequency Number density of defect clusters of size n Strength of drift term for clusters, by absorption of single defects Atomic volume Density of entity x Stress and components of stress Shear stress Value of shear stress that yields a dislocation velocity of 0.01 m/s Incubation time Eq. (7.95) Lifetime of dislocation loop

Subscripts c d i k L F N P

Dislocation core Dislocation Interstitial Critical cluster size Loop Frank loop Dislocation network Perfect loop

v 0

Vacancy Initial

Superscripts c cl s

Coalescence Clusters Single defects

Acronyms EDF IDF MCF MDF

Evaporating defect fraction Isolated point defect fraction Mobile cluster fraction Mobile defect fraction

337

338

7 Dislocation Microstructure

PBM PKA SFE SIA

Production bias model Primary knock-on atom Stacking fault energy Single interstitial atom

Problems 7.1 Draw billiard ball models of the extra half sheet of atoms which constitute the following dislocations: a) The a/2[110] edge dislocation in the (111) plane of the fcc lattice b) The a/2[111] edge dislocation on the (110) plane of the bcc lattice. 7.2 It is found experimentally that a certain material does not change in volume when subjected to an elastic state of stress. What is Poisson’s ratio for this material? 7.3 Determine the volume of a 10 cm diameter copper sphere that is subjected to a fluid pressure of 12 MPa. 7.4 Assuming that atoms are hard elastic spheres, show that Poisson’s ratio for a close-packed array of spheres is 1/3. 7.5 For a circular shaped disc lying on the (111) plane of an fcc crystal: a) Determine the energy as a function of the number of vacancies. b) How many vacancies could a spherical void have before it would spontaneously convert to a vacancy disc? 7.6 It is known that the amount of stored energy in a solid can be increased with the addition of dislocations. a) Calculate this energy for aluminum with a dislocation density of 108 cm−2 . b) It has also been suggested that this energy can be increased by application of a shear stress, σs . Given that the straight edge dislocations in part (a) are in the form of an equally spaced cubic shaped network, determine the shear stress, σs , needed to bow each dislocation segment into a half circle and calculate the increase in stored energy resulting. 7.7 Calculate the net density of edge dislocations in a thin simple cubic crystal with lattice parameter a = 2 ×10−8 cm if it is bent to have a radius of curvature of 10 cm. (The thickness of the crystal is no greater than 1 mm.) 7.8 In the circular shear loop shown in the figure below, let the x-axis be the direction of the Burgers vector shown in the drawing, the x-axis be in the plane of the loop but perpendicular to the direction of the Burgers vector, and the y-axis be perpendicular to the plane of the loop. Let θ be the polar angle of the circle measured from point A. At any point θ on the loop, the Burgers vector has an edge component be that is perpendicular to the dislocation line at that position and a screw component bs that is parallel to the line. a) Using the fact that the vector b with these components is constant (in magnitude and direction) at all points on the loop, derive expressions for be and bs as functions of θ .

Problems

339

b) Suppose a shear stress σxy is applied to the loop. Show that the resultant force on the dislocation line is always radially directed and has a magnitude σxy b.

7.9 Plot the stress fields surrounding an edge and screw dislocation as a function of θ . Specifically, plot the following: a) σxx , σyy and σxy vs. θ for an edge dislocation b) σxz and σyz vs. θ for a screw dislocation 7.10 For the dislocations in the figure below: a) Calculate the magnitude of the components of force on dislocation (2) due to dislocation (1). b) Repeat part (a) for angles of 0◦ , 30◦ , 45◦ and 90◦ . c) At θ = 30◦ , will dislocation (2) i) glide toward or away from dislocation (1)? ii) tend to climb up or down? Why?

340

7 Dislocation Microstructure

7.11 For the dislocations given in the sketch, find: a) The force on dislocation (2) due to dislocation (1) b) In which direction will dislocation (2) climb and/or glide? c) Describe the stress and temperature dependence of these two processes and under what circumstances each will contribute to creep.

(1) s = |001|, b = b|100| ¯ b = b|010| ¯ (2) s = |001|, 7.12 An edge dislocation having the properties s = k, and b = b j is on a plane x = X. Calculate the y-coordinates of the maxima and minima of the glide and climb forces (separately) that it would experience due to a fixed dislocation at the origin (s = k) for the following three cases: a) b = bi b) b = b j √ c) b = b(1/2i + 3/2 j). 7.13 An edge dislocation (1) with s = [001] and b = [100] is located a the origin of coordinate system. Another edge dislocation (2) with s = [001] and b = √a √ [ 2 2 0] is located a distance r away from (1) and 45◦ CCW from the xaxis. a) Calculate the glide and climb force on dislocation (2) due to dislocation (1). b) Make a graph of the force on dislocation (2) as a function of θ (for a given r) for 0 ≤ θ ≤ 2π . 7.14 Compute the local force on dislocation (2) due to dislocation (1) for the four examples of interaction between two perpendicular dislocations listed below: s1 = [001] ⎧ [100] ⎪ ⎪ ⎨ [100] b1 = [100] ⎪ ⎪ ⎩ [010]

s2 = [010] ⎧ [100] ⎪ ⎪ ⎨ [010] b2 = [001] ⎪ ⎪ ⎩ [010]

References

341

where the first dislocation passes through x = y = 0 and is parallel to the zaxis, and the second dislocation passes through x = X, z = 0 and is parallel to the y-axis. a) Show that the total force on dislocation (2) vanishes in all cases. b) If dislocation is able to flex, sketch the shape it is likely to assume, provided the fist dislocation passing through the origin remains straight.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23.

24. 25. 26. 27. 28. 29.

Weertman J, Weertman J (1964) Elementary Dislocation Theory. Macmillian, London Hull D, Bacon DJ (1984) Introduction to Dislocations. Pergamon, Oxford Friedel J (1964) Dislocations. Pergamon, New York Hirth JP, Lothe J (1982) Dislocations in Crystals, 2nd edn. Wiley Interscience, New York Reed-Hill RE, Abbaschian R (1994) Physical Metallurgy Principles, 4th edn. PWS, Boston Hull D, Bacon DJ (2001) Introduction to Dislocations, 4th edn. Butterworth Heinemann, Philadelphia Dieter GE (1976) Mechanical Metallurgy, 2nd edn. McGraw-Hill, New York, p 180 Osetsky YuN, Stoller RE, Matsukawa Y (2004) J Nucl Mater 329–333:1228–1232 Bacon DJ, Osetsky YuN, Stoller RE, Voskoboinikov RE (2003) J Nucl Mater 323:152– 162 Bacon DJ, Gao F, Osetsky YuN (2000) J Nucl Mater 276:1–12 Phythian WJ, Stoller RE, Foreman AJE, Calder AF, Bacon DJ (1995) J Nucl Mater 223:245–261 Osetsky YuN, Bacon DJ, Serra A, Singh BN, Golubov SI (2000) J Nucl Mater 276:65–77 Osetsky YuN, Bacon DJ, Singh BN, Wirth B (2002) J Nucl Mater 307–311:852–861 Stoller RE (2000) J Nucl Mater 276:22–32 Jenkins ML, Kirk MA (2001) Characterization of Radiation Damage by Transmission Electron Microscopy. Institute of Physics, Philadelphia, PA Kiritani M (1994) J Nucl Mater 216:200–264 Wirth BD, Odette GR, Marondas D, Lucas GE (2000) J Nucl Mater 276:33–40 Johnson RA (1967) Phil Mag 16(141):553 Jossang T, Hirth JP (1966) Phil Mag 13:657 Kelly BT (1966) Irradiation Damage to Solids. Pergamon, New York Zinkle SJ, Singh BN (1993) J Nucl Mater 199:173–191 Russell KC, Powell RW (1973) Acta Meta 21:187 Stoller RE, Odette GR (1987) In: Gerner FA, Packan NH, Kumar AS (eds) RadiationInduced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, pp 358–370 Golubov SI, Ovcharenko AM, Barashev AV, Singh BN (2001) Phil Mag A 81(3):643– 658 Ghoniem NM, Sharafat S (1980) J Nucl Mater 92:121–135 Semenov AA, Woo CH (2003) Phil Mag 813:3765–3782 Pokor C, Brecht Y, Dubuisson P, Massoud JP, Barbu A (2004) J Nucl Mater 326:19–29 Duparc AH, Moingeon C, Smetniansky-de-Grande N, Barbu A (2002) J Nucl Mater 302:143 Soneda N, Diaz de la Rubia T (1998) Phil Mag A 78(5):995

342

7 Dislocation Microstructure

30. Osetsky YN, Serra A, Victoria M, Golubov SI, Priego V (1999) Phil Mag A 79(9):2285 31. Garner FA, Kumar AS (1987) Radiation-Induced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, pp 289–314 32. Stoller RE, Odette GR (1987) In: Garner FA, Packan NH, Kumar AS (eds) RadiationInduced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, p 371 33. Eyre BL, Bullough R (1965) Phil Mag 12:31 34. Garner FA, Wolfer WG (1982) In: Brager HR, Perrin JS (eds) Effects of Radiation on Materials: 11th Conference, ASTM STP 782. American Society for Testing and Materials, West Conshohocken, PA, p 1073 35. Garner FA (1994) In: Frost BRT (ed) Materials Science and Technology, chap 6, vol 10A. VCH, New York, p 419 36. Zinkle SJ, Maziasz PJ, Stoller RE (1993) J Nucl Mater 206:266–286 37. Mansur LK (1994) J Nucl Mater 216:97–123 38. Edwards DJ, Simonen EP, Bruemmer SM (2003) J Nucl Mater 317:13–31

8 Irradiation-Induced Voids and Bubbles

The formation and growth of voids and bubbles is of intense interest for material performance in radiation environments at elevated temperature. The first observation of voids in irradiated metals was published by Cauthorne and Fulton in 1967 [1]. Voids can have a profound influence on material properties because solids undergo volumetric swelling when voids form and grow. It has been suggested that the US breeder reactor program experienced a setback of nearly a decade by this surprising observation, as scientists scrambled to understand this phenomenon and the consequences to reactor internals. Since that time, a great deal of effort has been expended toward understanding their formation and growth. Figure 8.1 shows examples of voids in irradiated stainless steel, aluminum and magnesium. Voids of this size and number density can cause tens of percent increases in volume, translating into significant changes in linear dimensions as well. The challenge of designing a reactor to accommodate swelling of this magnitude quickly becomes monumental. The formation and growth of voids shares much in common with bubbles. Yet because of their nature—a void is essentially an empty cavity—bubble mechanics are more complicated. It is by virtue of the fact that insoluble gases are formed by transmutation when certain metals are irradiated that drew attention to the subject of bubbles in irradiated metals. Under irradiation, it is possible for large numbers of inert gas bubbles to form, which significantly alter the physical and mechanical properties of metals. Fast and thermal spectrum reactors generate helium via transmutation, and the first wall of a fusion reactor is susceptible to bubble formation due to the high gas loading from reaction products in the plasma. Numerous examples exist in reactor systems where bubbles form and alter material properties, one of the most important being the structural materials of fission reactors. This chapter will address the theory of void and bubble nucleation and growth, along with elucidating the most important factors affecting these processes in reactor systems.

8.1 Void Nucleation The driving force for the formation of voids in solids is the supersaturation of vacancies due to irradiation defined by: Sv =

Cv , Cv0

(8.1)

344

8 Irradiation-Induced Voids and Bubbles

Fig. 8.1. Micrographs of irradiation-induced voids in (a) stainless steel, (b) aluminum (c) and (d) magnesium [2, 3]

where Cv0 is the thermal equilibrium concentration of vacancies. During irradiation, defects react to form clusters and the clusters either grow by absorption of defects of the same type, or shrink by absorption of defects of the opposite type. For a cluster of vacancies to grow into a void, there must be a net increase in the number of vacancies absorbed over the number of interstitials absorbed. Thus, we will be inter-

8.1 Void Nucleation

345

ested in the equilibrium void distribution function, ρ 0 (n) (where n is the number of vacancies in the void), which is developed by a supersaturation of vacancies in the solid. The distribution function gives the number of vacancy clusters in each size class. Under non-equilibrium conditions, there will be a net flux, J, of voids from one size class to the next larger size class. This is the nucleation current and is the quantity we are interested in finding. The presence of an inert gas in the nucleation process is then considered. 8.1.1 Equilibrium Void Size Distribution Analogous to the case of point defects (discussed in Chap. 4) and following the derivation in [4], the equilibrium void size distribution is determined from the change in Gibbs free energy of a system containing a distribution ρ 0 (n) of vacancy clusters: G = G0 + ∑ ρ 0 (n)Gn − kT ∑ ln wn , n

(8.2)

n

where G0 is the free energy of the perfect lattice, the second term is the work to form a void distribution, and the last term is the entropy contribution to the number of ways that the voids can be distributed in a lattice. The quantity Gn is the Gibbs free energy (reversible work) required to form a void of size n: Gn = Hn − T Sn = En + pn − T Sn ,

(8.3)

where En = the energy required to form a void of n vacancies n = volume change (= nΩ ) p = hydrostatic stress Sn = the excess entropy associated with the process wn = the number of ways of removing ρ 0 (n) voids of size n from the solid Neglecting the last two terms on the right, Gn reduces to Gn ∼ = En . For large values of n, the energy of the void can adequately be represented by the surface energy: EV = 4π R2V γ ,

(8.4)

where γ is the surface energy of the solid per unit area and RV is the void radius which is related to the number of vacancies in the void by: n=

4π R3V , 3Ω

(8.5)

where Ω is the atomic volume. The reader should note that the expression in Eq. (8.4) is the same as was developed in Eq. (7.58) and for the limiting case of a vacancy, Eq. (4.22). Equation (8.4) is, however, an approximation since the energy should properly include terms for the contraction of the surface and for the elastic energy stored in the solid (see Eq. (4.23)). Combining Eqs. (8.4) and (8.5)

346

8 Irradiation-Induced Voids and Bubbles

gives: En = (36πΩ 2 )1/3 γ n2/3 .

(8.6)

The last term in Eq. (8.2) is the product of the temperature and the mixing entropy. It can be obtained by calculating the number of ways in which voids can be distributed in a crystal containing N0 lattice sites per unit volume. The procedure is the same as that used for vacancies in Sect. 4.2 and results in: nρ (n) (N0 /n)! wn = . (N0 /n − ρ 0(n))!(ρ 0 (n))! 0

(8.7)

We now define the chemical potential of a void of size n as μn that is related to the Gibbs free energy by: ∂ G μn = . (8.8) 0 ∂ ρ(n) T,p,n

Substituting Eq. (8.7) into Eq. (8.2), using Stirling’s approximation for the factorial term in Eq. (8.7), and taking the derivative as required by Eq. (8.8) (∂ G = ∂ ΔG since ΔG = G − G0) gives:

0 ρ (n) μn = En + kT ln . (8.9) N0 We have neglected ρ 0 (n) compared to N0 because the void concentration is low. For monovacancies (n = 1), and Eq. (8.9) reduces to: Cv μv = Ev + kT ln . (8.10) N0 Since the equilibrium concentration of vacancies in a solid is given by: −Efv 0 Cv = N0 exp , kT substituting for N0 from Eq. (8.11) into Eq. (8.10) gives: Cv μv = kT ln = kT ln Sv . Cv0

(8.11)

(8.12)

The criterion for chemical equilibrium is that the chemical potential of reactants and products in the system be the same, i.e., n μv = μn .

(8.13)

Substituting Eqs. (8.9) and (8.12) into the criterion for chemical equilibrium, Eq. (8.13) gives:

ρ 0 (n) = N0 exp(n ln Sv − ξ n2/3) ,

(8.14)

8.1 Void Nucleation

347

where

ξ = (36πΩ 2)1/3

γ . kT

(8.15)

Substituting Eq. (8.15) into Eq. (8.14) and considering only the term inside the exponent, we have: n ln Sv − ξ n2/3 = n ln Sv −

(36πΩ 2 )1/3 γ n2/3 . kT

(8.16)

Expressing Eq. (8.14) as ρ 0 (n) = N0 exp(−ΔG0n /kT ) gives the following expression for ΔG0n : ΔG0n = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 ,

(8.17)

which is just the free energy change in the solid on forming a spherical void consisting of n vacancies on some particular site. A schematic of Eq. (8.17) is shown in Fig. 8.2 in which the free energy is plotted as a function of the number of vacancies in a void. Note that the first term decreases linearly with n while the second term increases as n2/3 . Accounting for the magnitude of the factors in each term, the resulting sum is a curve with a maximum at a value of n∗ . This is the critical size of a void embryo which must be achieved in order for the embryo to grow into a void. At the critical point, vacancy addition and removal both cause a reduction in

Fig. 8.2. Schematic illustration of ΔG0n , the free energy of formation of a spherical void consisting of n vacancies and the effect of thermal fluctuations on the critical size void embryo

348

8 Irradiation-Induced Voids and Bubbles

the Gibbs free energy of the system, so this is an unstable point. Above the critical size, addition of vacancies to the embryo causes a decrease in the free energy, which means that void growth is favored, while loss of vacancies causes an increase in the free energy, so this reaction is not favored. Note also that thermal fluctuations add an increment to the embryo size, pushing the critical size to a higher value, and thus making it more difficult to nucleate a stable void. 8.1.2 Void Nucleation Rate The nucleation rate of void embryos (consisting of n vacancies) can be described using the same formalism that was used to describe vacancy loop nucleation in Chap. 7 and developed in [5, 6, 7]. However, for the sake of continuity, that derivation will be repeated here for the case of void embryos. Recall from Eq. (7.74) that the nucleation rate of a void embryo of size n is given by: Jn = ρ 0 (n)βv (n)Z ,

(8.18)

where ρ 0 (n) is the concentration of voids of size n vacancies, βv (n) is the absorption rate and Z, the Zeldovich factor (defined in Sect. 7.6.1) and the void concentration is given by: −ΔG0n ρ 0 (n) = N0 exp , (8.19) kT where N0 is the number of sites on which voids can be formed, and ΔG0n is the change in free energy in the solid upon formation of the void and is given in Eq. (8.17). The value of ΔG0n for the critical void embryo size, ΔG0k (for embryo size nk ), is the activation barrier for void formation shown in Fig. 8.3 by the lower curve and is given as: 2/3

ΔG0k = −nk kT ln Sv + (36πΩ 2)1/3 γ nk

.

(8.20)

The void nucleation rate is the nucleation current given in Eq. (8.18). The void nucleation current, Jn , and activation barrier, ΔG0k , apply to the case where only vacancies are present. However, under irradiation, vacancies and interstitials are produced in equal numbers so the presence of interstitials must be accounted for. We now consider the case where interstitials can also impinge on voids. The analysis is similar to that just presented, but more complicated due to the introduction of another specie that will make void nucleation more difficult. Consider now, the nucleation of vacancy clusters on one particular kind of attractive site [4, 5, 6] such as the compressive stress field around a dislocation. The following assumptions are made: 1. The lattice is in thermal and dynamic equilibrium, which are minimally affected by displacement and thermal spikes. 2. Monovacancies and solvent monointerstitials are the only mobile point defects present.

8.1 Void Nucleation

349

Fig. 8.3. Schematic nucleation curves showing the various parameters which are important in void nucleation. ΔG0k is the activation barrier to nucleation if interstitials are not present, while ΔGk is the same quantity if interstitials are present during the nucleation process (after [6])

3. The defects obey dilute solution thermodynamics. 4. A steady state concentration of vacancies and interstitials exist. Assumption (1) is reasonable as thermal spike lifetimes are very short (10−12 s) and dynamical equilibrium should be attained in similar time intervals. Assumption (2) is generally not valid since gas atoms are often present and are known to play an important role in nucleation (treated in Sect. 8.1.3). Assumption (3) should be valid for low defect concentration (≤ 10−4 atomic fraction). The final assumption is a gross oversimplification since the microstructure continues to evolve with increasing dose causing sink strength, and therefore defect concentrations, to continually change. The following derivation of the void nucleation rate from kinetic considerations is similar to that for loops, in which the nucleation rate is expressed as the flux of clusters between adjacent size classes in a phase space of cluster size. A flux is the concentration times velocity or the product of concentration, jump frequency and jump distance. The flux between any two size classes, say n and n + 1, is: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) − βi(n + 1)ρ (n + 1) ,

(8.21)

where ρ (n) and ρ (n + 1) are the number of n-mer (voids containing a net of n vacancies) and (n + 1)-mers per unit volume. βv (n) is the rate of vacancy capture by a n-mer, αv (n + 1) and βv (n + 1) are the rates of loss and interstitial capture by a (n + 1)-mer. The first term in Eq. (8.21) represents an addition to the n + 1 size class by capture of a vacancy by a void of n-mer size class. The second term is a loss from the (n + 1)-mer size class by loss of a vacancy, and the third term is a loss from the (n + 1)-mer size class by capture of an interstitial. Interstitial emission is of low

350

8 Irradiation-Induced Voids and Bubbles Fig. 8.4. Illustration of the processes governing the flux of between adjacent void sizes in a phase space of void size

probability and is neglected. Figure 8.4 shows the various processes described by Eq. (8.21) in phase space. Setting J = 0 in Eq. (8.21) is equivalent to equilibrating the size classes since there is no net flux between size classes (as we did in Sect. 7.6). If we neglect interstitials, then we can write Eq. (8.21) as:

αv (n + 1) =

βv (n)ρ 0 (n) . ρ 0 (n + 1)

(8.22)

Combining Eqs. (8.21) and (8.22) gives:

0 ρ (n) βi (n + 1) Jn = βv (n) ρ (n) − ρ (n + 1) 0 + . ρ (n + 1) βv (n) Since ρ 0 (n) = N0 exp(−ΔG0n /kT ), then we note that: 0 ρ 0 (n) δ Gn = exp , 0 ρ (n + 1) kT

(8.23)

(8.24)

where δ G0n ≡ ΔG0n+1 − ΔG0n . We now define new functions of n, ρ (n) and δ Gn such that by analogy with Eq. (8.24):

ρ (n)

ρ (n + 1)

=

ρ 0 (n)

ρ 0 (n + 1)

+

βi (n + 1) = exp(δ Gn /kT ) , βi (n)

(8.25)

where

δ Gn = ΔGn+1 − ΔGn ,

(8.26)

βi (n + 1) in Eq. (8.25). βi (n) Using the expression in Eq. (8.25), we can re-write the equation for Jn in terms of ρ (n) by substituting Eq. (8.25) into Eq. (8.23) to give: ρ (n + 1) ρ (n) Jn = βv (n) ρ (n) − ρ (n + 1) . (8.27) ρ (n + 1)

and Δ Gn is not generally a free energy because of the term

8.1 Void Nucleation

Re-arranging Eq. (8.27) gives:

ρ (n) ρ (n + 1) Jn = −βv (n)ρ (n) − , ρ (n) ρ (n + 1) and noting that:

ρ (n) ρ (n + 1) ρ (n) − ∂ ρ (n) ρ (n + 1) ρ (n) = , Δn ∂n

351

(8.28)

(8.29)

gives: Jn = −βv (n)ρ (n)

∂ [ρ (n)/ρ (n)] , ∂n

(8.30)

which is the basic flux equation. Re-arranging Eq. (8.25) by taking the natural log of both sides and summing from j = 0 to n − 1 gives: n−1 n−1 δ G0j ρ ( j) βi ( j + 1) , (8.31) ∑ ln ρ ( j + 1) = ∑ − ln βv( j) + exp kT j=0 j=0 and:

ρ (n) ln ρ (0)

=

n−1

∑

j=0

δ G0j βi ( j + 1) + exp . − ln βv ( j) kT

(8.32)

We can identify two boundary conditions. The first is the quantity ρ (0), which may be evaluated by noting that as βi (n)/βv (n) → 0, ρ (0) = ρ 0 (0) and that ρ 0 (0) → N0 , is simply the number of nucleation sites per unit volume. Since N0 (and hence ρ (0)) is independent of void concentration, we can write: n−1 δ G0j ρ (n) βi ( j + 1) ln + exp = ∑ − ln ρ (0) βv ( j) kT j=0 (8.33) −ΔGn = . kT Since as βi (n)/βv (n) → 0, ρ (0) → ρ 0 (0) and ρ 0 (0) is just N0 , the number of nucleation sites per unit volume, we have then: −ΔGn ρ (n) = N0 exp , (8.34) kT and

ΔG0n = activation barrier without interstitials, ΔGn = activation barrier with interstitials.

352

8 Irradiation-Induced Voids and Bubbles

The upper curve in Fig. 8.2 shows ΔGn as functions of n. Note that ΔGn is larger than ΔG0k , and requires a larger void size due to the hindering effect of interstitials on the void nucleation process. The maxima in the two curves occur at nk , ΔG0k and nk , ΔGk . Now, the steady state void nucleation rate may be calculated from the expression for Jn in Eq. (8.30): Jk = Z βk ρk ,

(8.35)

which isthe rate at which voids escape over the potential barrier of height ΔGk in units of voids/cm3 s . The term βk , is the rate of single vacancy impingement on a void of size nk . If clusters are assumed to be spherical, then the vacancy impingement rate is expressed by the rate constant for point-defect absorption by spherical sinks, Eq. (5.99). Since void embryos are small, the capture rate is of mixed-control type in which both diffusion and reaction rate limitations are of comparable magnitude:

βv (n) =

4π RV DvCv , 1 + a/RV

(8.36)

were a is the lattice parameter, and assuming that the rate at which vacancies leave a void depends on the size of the void but not on the concentration of vacancies or interstitials or details of the dynamics. Note that for large voids, a/RV → 0 and βv (n) has a pure diffusion character. The term Z , analogous to Z but in the presence of interstitials, is:

Z = −

1 ∂ 2 ΔGn 2π kT ∂ n2

1/2 nk

.

(8.37)

The subscript indicates that the second derivative is to be evaluated at n = nk . Its value is the width of ΔGk at kT units below the maximum and is on the order of 0.05. The second derivative is found from Eq. (8.25) to be:

1 ∂ ΔG0 1 ∂ 2 ΔG0n 1 ∂ 2 ΔGn exp = , (8.38) kT ∂ n2 kT ∂ n2 kT ∂ n n n k

k

giving: ρk = N0 exp −ΔGk /kT ,

(8.39)

where ΔGk is determined by evaluating Eq. (8.33) at nk . Since the critical void nucleus size is taken as the maximum of the ΔGn curve, differentiating Eq. (8.17) and substituting the result into Eq. (8.33) permits evaluation of ΔGn . The maximum in ΔGn is determined by setting ∂ ΔGn /∂ n = 0 and

8.1 Void Nucleation

353

solving for n: nk =

36πγ 3Ω 2

3 , β (n) − β (n + 1) v i 3(kT )3 ln βv0 (n)

where Cv /Cv,0 nk

= βv (n)/βv0 (n).

Since RV =

3 nΩ 4 π

(8.40)

1/3 , the radius corresponding to

is: rk =

kT ln

2γΩ . βv (n) − βi(n + 1) βv0 (n)

(8.41)

Note that as βi → βv , rk → ∞, which says that if the capture rate for vacancies and interstitials is the same, then the critical void embryo size would need to be ∞. Figure 8.5 plots ρ (n) as a function of cluster size n for various values of βi /βv for Sv = 430 and T = 623 ◦C. Note the effect of increasing the interstitial arrival rate for a fixed vacancy arrival rate. With increasing arrival rate ratio, (βi /βv ) the slope of the distribution, dρ / dn decreases everywhere. The reason is that increasing the interstitial flux increases the fraction of embryos of a given size n which actually shrink to the next smallest size (n − 1), whereas to maintain the constrained distribution requires that the increased fraction be balanced by a decreased concentration of nuclei of size n relative to that of size (n − 1).

Fig. 8.5. Concentration of void embryos as a function of their size when the net flow of embryos is constrained to be zero. The parameters are the arrival rate ratios βi /βv , and the nucleation rates (in s−1 cm−3 ) of the unconstrained system. For this example, T = 623 ◦C and Sv = 430. Solid circles indicate the minima of n(x) (from [8])

354

8 Irradiation-Induced Voids and Bubbles Fig. 8.6. Nucleation rate as a function of the vacancy supersaturation. The parameters are the arrival rate ratios, βi /βv and the temperature (after [8])

Increasing the arrival rate ratio also shifts the minimum in the distribution ρ (n) to larger sizes and to lower concentrations. Since the nucleation rate is proportional to ρ (n), it decreases tremendously by the deepening and widening of the minimum in ρ (n) as the arrival rate ratio increases. The nucleation rate in Fig 8.5 decreases about 6 orders of magnitude as the arrival rate ratio is increases from 0 to 0.97. To obtain void nucleation as βi /βv approaches 1 requires higher vacancy supersaturation. The strong dependence of nucleation on vacancy supersaturation is affected only very slightly by the arrival rate ratio. Figure 8.6 shows that a factor of 10 increase in supersaturation causes the nucleation rate to increase from 1 to 1015 nuclei/cm3/s at 627 ◦C. The effect of temperature on the vacancy concentration, C∗ required to give a fixed nucleation rate is shown in Fig. 8.7 by the set of curves identified by the arrival rate ratios, βi /βv . Over most of the temperature range, C∗ increases with increasing temperature even though the supersaturation Sv = Cv /Cv0 decreases. Note that Cv is high at low temperature where the diffusion coefficient is small and there is not much loss. Cv is small at intermediate temperature where annihilation and loss to sinks is great. But Cv is high again at high temperature where Cv0 ∼ Cv . The parameter p is the probability per defect jump that the defect is annihilated at a sink. The values of p range from 10−7, typical of an annealed metal to 10−3 , which is typical of a heavily cold worked metal.

8.1 Void Nucleation

355

Fig. 8.7. Steady state vacancy concentration caused by a production rate of K0 = 10−3 atom fraction of defect pairs per second. The parameter p on the curves is the probability per jump that a defect is annihilated at existing sinks, such as dislocations. The curve labeled Cv0 is the thermal equilibrium concentration of vacancies. The set of curves labeled by the arrival rate ratio, βi /βv indicates the vacancy concentration required to give a nucleation rate of 1012 void nuclei/cm3 s. This nucleation rate is obtained at the temperature and vacancy concentration at the intersection of the curves under the conditions characterized by the curve parameters. The nucleation rate will be higher (lower) at temperatures below (above) the intersection temperature at fixed values of the parameters (after [8])

Figure 8.8 gives the steady state vacancy concentrations for several defect production rates, K0 and several nucleation rates J and for a sink-annihilation probability of 10−7 and an arrival rate ratio of 0.99. The intersection of the defect production rate and the nucleation rate provides the vacancy concentration at the temperature of the intersection. Higher vacancy production rates promote greater vacancy concentration and a higher nucleation rate. In summary, the void nucleation rate is a function of the height of the activation barrier. Inclusion of interstitials raises the activation barrier and reduces the nucleation rate. The critical void size radius for survival and growth as a void is a function of the activation barrier height with greater heights requiring larger critical void sizes. Nucleation rate is strongly increased by vacancy supersaturation and a reduced interstitial-to-vacancy arrival rate ratio. 8.1.3 Effect of Inert Gas Up to this point, we have assumed that a supersaturation of vacancies was sufficient to create a void embryo. It is well-known that inert gas atoms may act to

356

8 Irradiation-Induced Voids and Bubbles

Fig. 8.8. Steady state vacancy concentrations for several defect production rates and a sink annihilation probability p = 10−7 , and vacancy concentrations required for several nucleation rates J (in cm−3 s−1 ) at an arrival rate ratio of 0.99. Such nucleation rates are obtained at the indicated defect production rates at the temperature where the curves intersect (after [8])

stabilize a void embryo and assist in the nucleation process. In fact, there is evidence to suggest that gas atoms are always involved in the void nucleation process [6, 7, 8, 9, 10]. Hence, several theories have been proposed that involve void nucleation in the presence of inert and non-inert gases [9, 11]. Here we will consider a simple treatment [4, 9] of an immobile, inert gas, which is just as extension of the theory already developed. We will focus on helium since it is commonly produced by transmutation reactions in core structural materials. Helium is very immobile compared to vacancies or interstitials in the temperature range of void formation. Once helium is trapped by a void embryo, its return to the matrix is very unlikely. Therefore, nucleation in the presence of helium does not require us to consider the interaction between helium atoms, vacancies and in-

8.1 Void Nucleation

357

Fig. 8.9. Phase space for void nucleation showing movements of a void following point defect capture (βi , βv , βx ) or loss (αv , αx , Kxc ) (after [6])

terstitials in the formation of a void embryo. We may analyze the problem instead, by treating the inert gas atoms as sites for the formation of void embryos by migration of the point defects. In essence, this is a form of heterogeneous void nucleation rather than the homogeneous process described in Sect. 8.1.2. The phase space description of the gas-containing void behavior is similar to that given in Sect. 8.1.2 and in [6]. The void is assigned coordinates specifying its vacancy content (n) and the number of gas atoms it contains (x) (Fig. 8.9). The void moves in the +n direction by capturing vacancies and in the opposite direction by either thermal emission of vacancies or capture of interstitials: n˙ = βv0 n1/3 − αv − βi0 n1/3 ,

(8.42)

where βv0 and βi0 are the arrival rates of vacancies and interstitials to the void, αv is the emission rate of vacancies from the void and the factor n1/3 accounts for the dependence of the capture rate on the void size. Similarly, movement in the positive x-direction occurs by gas atom capture and in the opposite direction by re-solution of gas atoms (return of the gas atom to the matrix due to knock-out by irradiation) or by thermal emission of gas atoms: x˙ = βx0 n1/3 − αx − xKxc ,

(8.43)

where βx0 is the arrival rate of gas atoms, αx is the emission rate of gas atoms and Kxc is the rate of gas atom re-solution. For the case where the voids are in equilibrium with the vacancy and gas atom concentrations, the distribution of gas-filled void embryos containing n vacancies and x gas atoms is:

ρ 0 (n, x) = N exp

−ΔG0 (n, x) kT

,

(8.44)

where ΔG0 (n, x) is the free energy of formation of the gas-filled void, also referred to as an (n, x)-mer. For every (n − 1, x)-mer capturing a vacancy, a (n, x)-mer will

358

8 Irradiation-Induced Voids and Bubbles

emit a vacancy, and for every (n, x − 1)-mer capturing a gas atom, a (n, x)-mer will emit one. Then:

ρ 0 (n − 1, x)βv0(n − 1)1/3 = ρ 0 (n, x)αv (n, x) ,

(8.45)

ρ 0 (n, x − 1)βx0(x − 1)1/3 = ρ 0 (n, x)αx (n, x) ,

(8.46)

and

and substituting Eqs. (8.45) and (8.46) into Eq. (8.42) to eliminate αv (n, x) and αx (n, x) gives:

βi0 1 ∂ ΔG0 (n, x) n˙ 1 − 0 − exp βv kT ∂n

c 1 ∂ ΔG0 (n, x) xKx 0 1/3 1 − 0 1/3 − exp , x˙ = βx n kT ∂x βx n = βv0 n1/3

(8.47) (8.48)

which are the velocities of the void in (n, x) phase space. However, we are interested in the nucleation rate, which requires more development and is described in detail in [4]. We start with a distribution of gas-atom clusters, Mx , which is the number of gas-atom clusters per unit volume composed of x gas atoms. The total helium concentration in the solid is: M=

∑ xMx ,

(8.49)

x=1

and is determined by the helium production rate due to transmutation reactions. We assume that nucleation of voids occurs independently and simultaneously on each of the gas atom clusters characterized by Mx nucleation sites per unit volume. Nucleation is driven by the vacancy and interstitial supersaturation. In addition to heterogeneous nucleation at gas cluster sites, homogenous nucleation is assumed to occur also on the N0 lattice sites in the solid. The total nucleation rate is the sum of the contributions of the homogeneous and heterogeneous nucleation rates: J = Jhom + ∑ Jx ,

(8.50)

x=1

where Jhom is given by Eq. (8.35). In order to obtain the total nucleation rate, we need to determine the heterogeneous nucleation rate Jx on the Mx gas cluster sites. The distribution of helium void embryos containing n vacancies and x gas atoms, ρ 0 (n, x) is governed by the reaction: nv = vnx ,

(8.51)

where vnx denotes a void consisting of n vacancies and x gas atoms. Since helium is immobile, there is no chemical reaction expressing the equilibration of gas atoms

8.1 Void Nucleation

359

between the voids and the bulk. The criterion of chemical equilibrium is then: n μv = μnx ,

(8.52)

and the chemical potential of a void with n vacancies and x gas atoms is:

μnx =

∂G . ∂ ρ 0 (n, x)

(8.53)

The formulation of the total Gibbs free energy for the gas-vacancy cluster is similar to the analysis presented earlier for vacancies alone. Analogous to Eq. (8.2) for voids, the total Gibbs free energy is: G = G0 + ∑ ∑ ρ 0 (n, x)Gnx − kT ln wnx . (8.54) x

n

As before, wnx is the number of ways of arranging ρ 0 (n, x) voids on Mi sites: ) * Mx (Mx − 1) . . . Mx − ρ 0 (n, x) − 1 Mx ! wnx = = . 0 0 [ρ (n, x)]! [Mx − ρ (n, x)]![ρ 0 (n, x)]! (8.55) Using Eq. (8.55) in Eq. (8.54) and using Eq. (8.54) to determine the chemical potential as given in Eq. (8.53) yields:

0 ρ (n, x) μnx = Gnx + kT ln . (8.56) Mx The reversible work to form a void embryo from n vacancies and x gas atoms is [4, 12]: MHnΩ Gnx = (36πΩ 2 )1/3 γ n2/3 − xkT ln . (8.57) xkT The first term is the work to create a gas-free void consisting of n vacancies, and is the same as that given in Eq. (8.6) for void formation. The second term is work to move the helium from the solid into the void. H in the second term is the Henry’s law constant for the dissolution of helium in the metal. The expressions for Gnx in Eq. (8.57) is substituted into the expression for the chemical potential of a void with n vacancies and x gas atoms, Eq. (8.56). Using the equality in Eq. (8.52) with μv given by Eq. (8.12) and solving for ρ 0 (n, x)gives:

MHnΩ 0 2/3 ρ (n, x) = Mx exp n ln Sv − ξ n + x ln . (8.58) xkT which is identical to Eq. (8.14) except for the extra term in the exponent and the preexponential factor. In fact, for x = 0 and Mx = N0 the result reduces to Eq. (8.14).

360

8 Irradiation-Induced Voids and Bubbles

Fig. 8.10. Plot of the free energy of void formation as a function of the number of vacancies (n) and the number of gas atoms (x) in the void. Conditions are: Sv = 600, p0 = 507 MPa, T = 500 ◦C, γ = 1 J/m2 (after [12])

Using Eq. (8.44) with Mx substituted for N0 gives: ΔG0 (n, x) = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 − xkT ln

MHnΩ xkT

.

(8.59)

Figure 8.10 shows the free energy of void formation as a function of n and x. The intercept of this surface at x = 0 (no gas) corresponds to the βi /βv = 0 curve in Fig. 8.5 in which ρ is plotted as a function of n in Eq. (8.34), ρ (n) = N0 exp(−ΔGk /kT ), and for βi /βv = 0, then ΔGn = ΔG(n, x = 0). Note that gas atoms in the void reduce the energy barrier for nucleation below that value characteristic of gas-free voids. The saddle point on the surface shown in Fig. 8.10 occurs at n = 11 and x = 6. The plot, however, does not include interstitials (as would a plot of ΔGn ), which are included in the analysis in exactly the same manner as in the case of homogeneous nucleation. The determination of the nucleation rate is done in the same manner as for homogeneous nucleation, resulting in a nucleation current: Jk,x = Zx βkx ρk (n, x) ,

(8.60)

8.1 Void Nucleation

361

Fig. 8.11. Void nucleation rates (J) on helium atom clusters and the homogeneous nucleation rate (Jhom ) as functions of vacancy supersaturation at 500 ◦C. Total helium content of 10 ppm (after [13])

where Zx =

−1 ∂ 2 ΔG (n, x) 2π kT ∂ n2

1/2 ,

(8.61)

ρ (n, x) = Mx exp(−ΔG (n, x)/kT ) ,

(8.62)

n=nk

and ΔG (n, x) = kT

0 βi 1 ∂ ΔG0 (n, x) ln + exp , ∑ βv0 kT ∂n x=0 n

(8.63)

and the values of zk and ρ (nk , x) are evaluated at the critical void size, nk , and βkx is the rate of impingement of vacancies on a critical size void. To determine the nucleation rate on the gas-atom clusters in the metal, we must estimate the distribution of the available gas (M atoms/cm3 ) among the various clus−(x+1) ter sizes. For simplicity, the distribution Mx = M1 is assumed. This distribution must satisfy Eq. (8.49). Figure 8.11 shows the results of calculations based on Eq. (8.60) to Eq. (8.62) and Eq. (8.60) for M equivalent to 10 ppm helium (equivalent to the amount of helium expected in stainless steel cladding after a fluence of 5 ×1022 n/cm2 ). Note that in the regime of vacancy supersaturation expected in a reactor, heterogeneous nucleation on helium-atom clusters far outweighs homogeneous nucleation. This behavior constitutes theoretical confirmation of the oftenobserved enhancement of void nucleation of helium. The relative importance of

362

8 Irradiation-Induced Voids and Bubbles

homogeneous and heterogeneous nucleation shifts according to the helium concentration because Jhom (n) is proportional to N0 whereas Jx (n) is proportional to Mx . At low fluence, homogeneous nucleation is dominant because there is not enough helium to drive heterogeneous nucleation. However, since Jhom is quite low, no voids are observed until sufficient helium has been generated by transmutation reactions to give the high heterogeneous nucleation rate. This incubation time is physically the relaxation time for the approach to steady state after a step increase in supersaturation. For void formation with or without the presence of gas:

τ = (2βk Z )−1 .

(8.64) 1022 n/cm2

This value is equivalent to a fluence of for fast reactor irradiation conditions. In summary, the effect of gas atoms is to substantially increase the void nucleation rate by lowering the critical radius for a stable void embryo below that for a gas-free void. Therefore, gas atom introduction into the lattice (either by transmutation or accelerator injection) promotes the formation of voids relative to the pristine lattice. 8.1.4 Void Nucleation with Production Bias The kinetic equation for dislocation loop evolution under cascade damage conditions was developed in Sect. 7.6.3 for interstitial clusters. We can use the same formulation with some changes to the terms to make the formulation specific to void nucleation [14]. Given that the number of vacancies in a spherical void can be written as: 1/3

dnv 3nv = 2 [DvCv − DiCi − DvCv0 ] dt a V 0 Cv = Cv exp(2γΩ /kT RV ) ,

(8.65) (8.66) 1/3

where a = (3Ω /4π )1/3, nv is the number of vacancies in a void, Rv = anv and Ω is the atomic volume, the drift velocity, F(n) (from the Fokker–Planck treatment) is now a single term equal to the RHS of Eq. (8.65). The diffusive spread, described by the term D(n) is a sum of contributions due to single defect jumps, cascades, and vacancy emission as: D(n) = Ds (n) + Dc (n) + De (n) ,

(8.67)

where 3n1/3 [Dv (Cv − Cv0) + DiCi ] , 2a2 + 2, + , Kieff Ndi2 3n2/3 Kveff Ndv c + , D (n) = 4a kv Ndv ki Ndi Ds (n) =

De (n) =

9DvCv0 n2/3 , 2a2

(8.68) (8.69) (8.70)

8.1 Void Nucleation

/

363

0

2 and K eff j is the effective generation rate of free point defects, Nd j and Nd j are the average number and the average square number of free point defects generated in a single cascade, respectively, and k2j is the total sink strength for point defects of the type j. The solution to the general kinetic equation is similar to that for the case of interstitial clusters and is given in [14]. For the case of small critical vacancy size, the solution is: 1/2 β (DvCv − DiCi ) ∼ Pm = (n0 − nv 0 ) 1/3 6π Rcr ncr DiCi (1 + dncr ) 2/3 2/3 η (β /Rcr )ncr − n0 × exp − , (8.71) 1/3 1 + 1/(d encr ) + d c /d e

where n0 is the initial void embryo size (generally ∼ 4 vacancies), nv0 is a minimum size of a void embryo below which it is no longer a void (generally ∼ 2–3 vacancies), d = d c + d e , β = 2γΩ /kT and Rcr and ncr are the size and vacancy content of the critical size embryo. The term Rcr is determined from Eqs. (8.65) and (8.66) under that condition that a void will grow if it receives a net vacancy flux (DvCv > DiCi ): Rcr =

β DvCvV , DvCv − DiCi − DvCvV

(8.72)

and R(n) = an1/3. The terms d c and d e are strengths of the diffusive spread for clusters and for vacancy emission relative to single point defects: dc =

Dc (ncr ) 1/3 s ncr D (ncr )

,

de =

De (ncr ) 1/3 s ncr D (ncr )

,

(8.73)

and the function η has a value between 0.55 and 0.84. Application of Eq. (8.71) for various values of d c and d e and for a void embryo size of 4 vacancies leads to nucleation probabilities in the range 10−6 to 10−4 for critical vacancy clusters of size ∼ 100 vacancies (Fig. 8.12). The nucleation rate is then: J∼ =

Kcleff Pm , Nd

(8.74)

where Kcleff is the effective generation rate of point defects in cluster and free form and Nd is the average total number of point defects generated in a single cascade and εi is the fraction of interstitials produced in cascades in the form of immobile clusters. Figure 8.13 shows the void nucleation rate calculated for annealed copper compared with experimental data at 250, 300 and 350 ◦C and different surface energies, γs and for different values of d e . In terms of void nuclei created cm−3 s−1 , the nucleation rate is in the range 1015 to 1018, which is larger than what was predicted by conventional nucleation theory. Thus, the effect of production bias is to increase the nucleation rate.

364

8 Irradiation-Induced Voids and Bubbles

Fig. 8.12. Nucleation probability plotted from Eq. (8.71) for initial void size of four vacancies and minimum size of one vacancy and for different values of d c and d e vs. the critical void (DvCv − DiCi )[1 − exp(−β /Rcr )] size, ncr . The term ν = (after [14]) DiCi

Fig. 8.13. Void nucleation rate vs. irradiation temperature for the case of copper under a displacement rate of 10−8 dpa/s (after [14])

8.2 Void Growth

365

8.2 Void Growth Having determined expressions for the rate at which voids are nucleated in the solid, we now turn to determining the rate at which the void nuclei grow into stable voids. As mentioned earlier, we will assume that the nucleation and growth stages are separated in time and that only when the void embryos are established does growth begin. Of course, this is a simplification of the true in-reactor situation in which the growth of stable nuclei is occurring simultaneously with nucleation. Void growth is determined by solving the point defect balance equations developed in Chap. 5. These equations provide the vacancy and interstitial supersaturations that drive the nucleation and growth processes. The concentrations of vacancies and interstitials in the solid are determined by equating the rates of defect production and removal by all mechanisms. By doing so, the time derivatives are removed and the resulting solution has the form of a steady state solution. However, since the defect concentrations are changing with time (dose), the steady state solution is valid over only short time periods, and is termed quasi-steady state. The quasi-steady state solution has value because the changes in sink strength due to microstructure evolution is slow compared to the response time of the defect populations. So in essence, the problem can be solved by assuming an initial condition that properly characterizes the sink strengths, solving the point defect balance equations for those sink strengths, then updating the sink strengths and iterating. Rates of production and removal are assumed to be uniform throughout the metal. Clearly, strong gradients will exist close to the sink. But they can be neglected by homogenizing or smearing the sink strengths, that is, by replacing discrete sinks by spatially uniform absorbers of point defects so that the aggregate effect on defect absorption is the same in the homogenized sink case as in the heterogeneous sink case. The sink strengths are those described in Chap. 5. Void growth is then calculated according to rate theory as developed by Brailsford and Bullough [14] subject to the following simplifications: 1. Discrete sinks are replaced by a continuous or smeared distribution of sinks. 2. Each sink is given a strength so that the current of defects to the smeared sink is the same as the current to the actual sinks in the real material. 3. Steps 1 and 2 remove the spatial dependence of Cv and Ci and the point defect balance equations become:

∂ Cv = K0 − ∑ Avj − Riv ∂t j ∂ Ci j = K0 − ∑ Ai − Riv , ∂t j

(8.75)

where the first term on the right is the production rate of vacancies and interstitials, the second term is the loss rate to all sinks and the last term is the loss rate due to vacancy–interstitial recombination. 4. Vacancy and interstitial concentrations, Cv and Ci are calculated from Eq. (8.75). The change in sink strength due to the flow of defects to the sink is calculated,

366

8 Irradiation-Induced Voids and Bubbles

and the process, starting with step 1, is iterated in order to advance in time and dose. Reaction rate constants for defect–sink reactions and sink strengths for the relevant sinks were determined in Chap. 5 and summarized in Table 5.1. Recall that sinks are classified as neutral (voids, grain boundaries, incoherent precipitates), biased (dislocation network and dislocation loops) or variable biased (coherent precipitates and over/undersized solutes). For all sink types, the defect absorption rate is proportional to the diffusion coefficient of the point defect and the difference in defect concentration between the bulk and the sink surface. With the exception of dislocation loops, the interstitial concentration at the sink surface is insignificant compared to the bulk value and may be neglected. In the case of vacancies, their concentration at the network dislocation core is maintained at the equilibrium concentration. For voids and loops, the vacancy concentration at the sink surfaces must also be determined. Once the sink strengths and the defect concentrations at the sink surfaces are all known, then we can determine the net absorption rate of defects by void nuclei and use this information to determine the growth rate of the voids. 8.2.1 Defect Absorption Rates and Concentrations at Sink Surfaces We seek to determine expressions for the absorption rates of defects for each of the relevant of sinks, categorized according to sink type. The general form of the absorption rate is: AXj = kX2 D j (C j − CXj ) = kX2 D jC j − LXj ,

(8.76)

where AXj is the absorption rate of defect j by sink X, kX2 is the strength of sink X, D j is the diffusion coefficient of defect j, C j and CXj are the bulk concentration and sink surface concentration of defect j, and LXj is the thermal emission rate of defect j by sink X. Note that for neutral sinks, the sink strengths are dependent only on the character of the sink and not the defect. This is the advantage of writing the loss terms using sink strengths rather than reaction rate constants. Neutral Sinks The loss rate of point defects to voids can be written as: 2 V 2 V AV v = kV Dv (Cv − Cv ) = kV DvCv − Lv V 2 Ai = kV DiCi ,

(8.77)

2 is the sink strength of a void given in Table 5.1, CvV is the vacancy concenwhere kV tration at the void surface, LV v is the thermal emission rate of vacancies at the sink surface and all voids are assumed to be the same size. The loss rate of defects to incoherent precipitates is: 2 AIP v = kIP DvCv 2 AIP i = kIP DiCi ,

(8.78)

8.2 Void Growth

367

and to grain boundaries the rate is: 2 Agb v = kgb DvCv gb

2 Ai = kgb DiCi ,

(8.79)

where the sink strengths are given in Table 5.1, and thermal emission terms have been neglected. Among Eqs. (8.77), (8.78), and (8.79), the term that is yet to be determined is the vacancy concentration at the void surface, CvV . This is done as follows. Recall from Eq. (4.14) that the thermal equilibrium concentration of vacancies in a solid is: Sf Hf 1 0 exp , Cv = exp Ω k kT where Hf = Ef + pΩ ,

(8.80)

and the pΩ term was neglected for single vacancies embedded in the lattice. This simplification does not hold in the solid surrounding a void where forces such as surface tension, pressure due to gas in the void and an external hydrostatic stress are acting. For example, the existence of a void surface produces a surface tension that can be determined, using Fig. 8.14, as follows: 2π rγ sin θ ∼ 2π rγ 2π r γ r 2γ Force = = , (8.81) θ = = unit area A π r2 π r2 R R where the approximation is that sin θ is replaced with θ for small θ . Hence, the p term in Eq. (8.80) becomes: 2γ , (8.82) R where the minus sign enters because the surface tension acts in an inward direction to shrink the void. The vacancy concentration at the void surface then becomes: Sf 1 Ef pΩ V Cv = exp exp − exp − , (8.83) Ω k kT kT p=−

where: Cv0 =

Sf 1 Ef exp exp − , Ω k kT

and substituting for pΩ from Eq. (8.82) gives: 2γΩ CvV = Cv0 exp , RkT and Eq. (8.77) becomes:

2γΩ V 2 0 Av = kV Dv Cv − Cv exp . RkT

(8.84)

(8.85)

(8.86)

368

8 Irradiation-Induced Voids and Bubbles Fig. 8.14. Schematic of the surface tension on a void of radius r

Biased Sinks The defect loss rate to network dislocations is given by: 2 2 Adv = kvd Dv (Cv − Cv0 ) = kvd DvCv − Ldv 2 Adi = kid DiCi ,

(8.87)

where the sink strengths are given in Table 5.1 and the term Cv0 is the thermal equilibrium concentration of vacancies. For interstitial dislocation loops, the loss term is: 2 2 Dv (Cv − CvL ) = kvL DvCv − LLv ALv = kvd 2 2 ALi = kid Di (Ci − CiL ) = kiL DiCi − LLi ,

(8.88)

where the sink strengths are the same as for network dislocations since the dislocation core is the same. However, the defect concentration at the sink surface is different from the thermal equilibrium value because addition of a vacancy or an interstitial to the dislocation loop contracts or expands, respectively, the size of the loop and this requires a change in energy. The concentration of vacancies and interstitials in equilibrium with a loop are CvL and CiL , respectively. Following the analysis in [4] the defect concentration in equilibrium with the loop is determined by considering the Gibbs free energy of a piece of metal containing nv vacancies and ni interstitials at concentrations CvL and CiL , and a single interstitial loop containing mi interstitials: G = G0 + EL(mi ) + nv μv + ni μi ,

(8.89)

where G0 is the free energy of solid without the loop but with Cv and Ci defects, EL (mi ) is the energy of the loop, and μi,v are the chemical potentials of interstitials and vacancies in the solid. For the system to be in chemical equilibrium, the transfer of point defects between the solid and the loop must cause no change in the free energy of the system: dEL δG = δ mi + μ v δ n v + μ i δ n i = 0 , (8.90) dmi

8.2 Void Growth

369

and

δ mi = δ n v − δ n i ,

(8.91)

since the number of interstitials in the loop must come from the bulk. Eliminating δ mi from Eqs. (8.91) and (8.92) gives: dEL dEL δ nv − δ n i + μv δ n v + μi δ n i = 0 . (8.92) dmi dmi Since changes in vacancy and interstitial concentrations are arbitrary and independent of each other, the coefficients of both changes are set equal to zero, leading to: dEL + μv = 0 dmi dEL − μi = 0 . dmi

(8.93)

From Eq. (8.12), the chemical potential of vacancies and interstitials in a solid with concentrations CvL and CiL is:

μv = kT ln

CvL Cv0

CL μi = kT ln i0 . Ci

(8.94)

For vacancies and interstitials in equilibrium: CvLCiL = Cv0Ci0 ,

(8.95)

or from Eq. (8.94):

μv = − μi .

(8.96)

Combining Eqs. (8.93) and (8.94) for vacancies and then for interstitials, yields: dEL / dmi L 0 Cv = Cv exp − kT (8.97) dE / dmi L L 0 Ci = Ci exp . kT Using Eq. (7.62) for the energy of a Frank loop: √ 1/2 √ 3a2 mi 3a2 mi 2 +π γSFE , EL = 2 π μ b 4π 4π

370

8 Irradiation-Induced Voids and Bubbles

and dropping the second term for simplicity, then dEL / dmi becomes:

Θ dEL = √ , dmi 2 mi √ 1/2 3a2 2 . Substituting into Eq. (8.97) yields: where Θ is 2π μ b 4π Θ L 0 Cv = Cv exp − √ 2 mi kT Θ L 0 Ci = Ci exp √ . 2 mi kT

(8.98)

(8.99)

Note that the vacancy concentration in equilibrium with an interstitial loop is less than the equilibrium vacancy concentration in the solid while the reverse is true for interstitials. The absorption rates of vacancies and interstitials at loops then becomes, from Eq. (8.88):

Θ L 0 Av = zv Dv ρL Cv − Cv exp − √ 2 mi kT

(8.100) Θ L 0 Ai = zi Di ρL Ci − Ci exp √ . 2 mi kT Variable Biased Sinks The sink strengths for variable biased sinks are given in Eq. (5.117) and are: 2 = 4π RCP ρCPYv kvCP 2 kiCP = 4π RCP ρCPYi ,

where Yv,i are sink strengths for coherent precipitates for vacancies and interstitials and the loss rate of point defects to coherent precipitates is: 2 ACP v = kvCP DvCv = 4π RCP ρCPCvYv 2 ACP i = kiCP DiCi = 4π RCP ρCPCiYi .

(8.101)

8.2.2 Point Defect Balances Now that we have expressions for the absorption rates of defects for each type of sink, we can construct the steady state, point defect balances for the solid under irradiation: K0 − ∑ Avj − Riv = 0 j

K0 − ∑ Aij − Riv = 0 , j

(8.102)

8.2 Void Growth

371

and in the most general form: K0 − kv2 Dv (Cv − CvX ) − KivCvCi = 0

(8.103)

K0 − ki2 Di (Ci − CiX ) − KivCvCi = 0 , where kv2 and ki2 are the total sink strengths for vacancy and interstitial loss: 2 2 2 2 2 2 + kvIP + kvgb + kvN + kvL + kvCP kv2 = kvV

(8.104)

2 2 2 2 2 2 ki2 = kiV + kiIP + kigb + kiN + kiL + kiCP ,

and the CvX and CiX are concentrations of vacancies and interstitials at the sink surface. Now, since defect production rates and recombination rates in Eq. (8.103) are equal and there is no net accumulation of point defects at coherent precipitates, then:

∑ Avj = ∑ Aij , j

(8.105)

j

or gb

IP gb d L V IP d L AV v + Av + Av + Av + Av = Ai + Ai + Ai + Ai + Ai ,

(8.106)

and therefore: 2 2 2 2 2 2 N L + kvIP + kvgb + kvN + kvL + kvCP )DvCv − LV (kvV v − Lv − Lv 2 2 2 2 2 2 = (kiV + kiIP + kigb + kiN + kiL + kiCP )DiCi − LLi .

(8.107)

where the L terms are the thermal emission of the defect from the sink. Substituting in for the expressions for sink strength and thermal emission from the respective equations in Chaps. 5 and 7 gives:

2γΩ 0 + zv ρN Dv Cv − Cv0 + 4π RCPρCP DvCvYv 4π RV ρV Dv Cv − Cv exp RkT

Θ 0 + zv ρL Dv Cv − Cv exp − √ 2 mi kT = π RV ρV DiCi + zi ρN DiCi + 4π RCPρCP DvCvYi

Θ 0 + zi ρL Di Ci − Ci exp √ , 2 mi kT (8.108) where terms for grain boundaries and incoherent precipitates are neglected for simplicity. Since the thermal equilibrium interstitial concentration, Ci0 is extremely small, the thermal emission of interstitials from loops can be neglected.

372

8 Irradiation-Induced Voids and Bubbles

8.3 Void Growth Equation Now that we have determined the absorption rate of defects for each sink in the solid, we focus on the void with the objective of developing an expression describing its rate of growth. The void growth equation has its origins in the net flux of vacancies to a void embryo. The net rate of absorption of vacancies by a void is: V V V V AV , (8.109) net = Av − Ai = 4π RDv Cv − Cv − 4π RDi Ci − Ci where R = void radius (we have dropped the subscript V for simplicity) Cv,i = vacancy/interstitial concentration in the solid CvV = vacancy concentration at the void surface, and thermal emission of interstitials from loops is neglected The rate of change in volume of the void is just the net absorption rate times the defect volume, Ω : dV = 4π RΩ Dv Cv − CvV − DiCi , dt

(8.110)

and since, 4 V = π R3 , 3

(8.111)

we obtain the common form of the void growth equation: dR Ω = R˙ = Dv Cv − CvV − DiCi . dt R

(8.112)

Our objective is to determine an expression for the void growth equation, which amounts to determining the values for Cv ,Ci , and CvV . The general solution procedure is thus to solve the point defect balance equations in Eq. (8.75) for Cv and Ci at some initial value of the void radius, R(0) and then to use those values of Cv and Ci in Eq. (8.112) to increment the void size from R to R . Since sink strength changes with void size, updated values of Cv and Ci must be obtained for the next void growth increment. The process is then iterated to describe the change in void size with time or dose. This process can be carried out numerically and with small time steps in order to minimize the time increment over which the sink strengths are assumed to be constant. In solving for void size in this way, changes to the microstructure can also be incorporated at the time step boundaries. While a numerical solution of the void growth equation will produce the most accurate result, it provides no insight into the governing processes during void growth. Brailsford and Bullough [15] inserted the solution of Eq. (8.75), into Eq. (8.112) to obtain an approximate analytical result that provides an excellent tool for understanding the parameters governing void growth. Mansur [5, 16] advanced the analysis to develop expressions for the dependence on critical parameters affecting void growth. We begin by returning to the point defect balance equations

8.3 Void Growth Equation

373

at steady state in order to determine the bulk concentrations of vacancies and interstitials, Cv and Ci . Setting the time rate of change of the vacancy and interstitial concentrations equal to zero in Eq. (8.75) gives: K0 − ∑ Avj − Riv = 0 j

K0 − ∑ Aij − Riv = 0 ,

(8.113)

j

or K0 − KivCiCv − KvsCvCs = 0 K0 − KivCiCv − KisCiCs = 0 ,

(8.114)

with solutions:

2 C2 1/2 K0 Kvs Kvs −KisCs s + + 2Kiv Kiv Kis 4Kiv

1/2 K 2 C2 K0 Kis −KvsCs Ci = + + is s , 2Kiv Kiv Kvs 4Kiv

Cv =

(8.115)

where Cs is the sink concentration. Using Table 5.1 to write the reaction rate constants for vacancies and interstitials at sinks as sink strengths gives:

1/2 −ki2 K0 kv2 Di kv2 D2v + + 2Kiv Kiv ki2 Dv 4Kiv

1/2 K0 ki2 Dv ki2 D2i −kv2 Ci = + + . 2Kiv Kiv kv2 Di 4Kiv

Cv =

(8.116)

Defining:

η=

4Kiv K0 , Di Dv kv2 ki2

(8.117)

and kv2 = zv ρd + 4π RρV + 4π RCPρCP ki2 = zi ρd + 4π RρV + 4π RCPρCP ,

(8.118)

where, for simplicity, we have neglected grain boundaries, incoherent precipitates and bias factors on voids and coherent precipitates, and the network dislocations and dislocation loops are represented by a single term with density ρd = ρN + ρL . Using Eqs. (8.117) and (8.118), then Eq. (8.116) can be written as: Di ki2 (η + 1)1/2 − 1 Cv = 2Kiv (8.119) Dv kv2 1/2 (η + 1) − 1 . Ci = 2Kiv

374

8 Irradiation-Induced Voids and Bubbles

The void growth rate from Eq. (8.112) can be written in the form: R˙ = R˙ 0 X(η ) ,

(8.120)

where K0 (zi − zv )ρd Ω R(zv ρd + 4π RρV)

. R˙ 0 = (zi − zv )ρd zi ρd + 4π RρV + 4π RCPρCP 1 + zv ρd + 4π RρV

(8.121)

Equation (8.121) can be simplified by dropping the last term in the square brackets in the denominator, since the difference (zi − zv ) is small, giving: R˙ 0 =

K0 (zi − zv )ρd Ω . R(zv ρd + 4π RρV)(zi ρd + 4π RρV + 4π RCPρCP )

(8.122)

This growth term is independent of temperature and is proportional to the dislocation bias for interstitials (zi − zv ) and the defect production rate. Note that R˙ 0 is: – – –

Independent of temperature Proportional to the dislocation bias (zi − zv ) Proportional to the defect production rate, K0

The term X(η ) is given by: X(η ) = F(η ) − 2ζ ,

(8.123)

where: F(η ) =

2 (η + 1)1/2 − 1 , η

(8.124)

and η is a dimensionless parameter defined in Eq. (8.117). Substituting Eq. (8.123) into Eq. (8.120) gives: R˙ = R˙ 0 F(η ) − 2R˙ 0 ζ .

(8.125)

The quantity η in the function F(η ) can be simplified by substituting in for kv2 and ki2 from Eq. (8.104) (or Table 5.1), giving:

η=

4Kiv K0 . (8.126) Di Dv (zi ρD + 4π RρV + 4π RCPρCP )(zv ρd + 4π RρV + 4π RCPρCP )

Using the approximation that zi ∼ = zv , and eliminating Kiv by using Eq. (5.57) gives:

η=

4ziv K0 Ω . Di Dv (zρD + 4π RρV + 4π RCPρCP )2

(8.127)

The expression for η is substituted into Eq. (8.124) to obtain an expression for F(η ). This function describes the effect of homogeneous recombination on void growth

8.3 Void Growth Equation

375

(Fig. 8.15). When recombination is negligible Kiv → 0 and η → 0, and F → 1, or lim F(η ) = 1. η →0

Turning now to the second term in Eq. (8.125), we define for simplicity: R˙ th = −2R˙ 0ζ ,

(8.128)

so that Eq. (8.125) can now be written as: R˙ = R˙ 0 F(η ) + R˙ th ,

(8.129)

The term ζ is a function of temperature and is expressed as:

ζ = ζ (T ) =

Dv (zv ρd + 4π RρV) [zi ρd + 4π (RρV + RCP ρCP )] 2K0 (zi − zv ) [zv pd + 4π (RρV + RCP ρCP )] (8.130) ) V V * V 0 L × 4π RCPρCPCv + zv ρN Cv − Cv + ρL Cv − Cv .

so that: −2Dv (zv ρd + 4π RρV) [zi ρd + 4π (RρV + RCP ρCP )] R˙ th = −2R˙ 0 ζ = 2K0 (zi − zv )ρd [zv ρd + 4π (RρV + RCP ρCP )] K0 (zi − zv )ρd Ω R(zv ρd + 4π RρV)

× (zi − zv )ρd zi ρd + 4π RρV + 4π RCPρCP 1 + zv ρd + 4π RρV × 4π RCP ρCPCvV + zv ρN CvV − Cv0 + ρL CvV − CvL .

(8.131)

By approximating zi ∼ = zv , numerous terms in Eq. (8.131) cancel, leaving: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP ) × 4π RCP ρCPCvV + zv ρN CvV − Cv0 + ρL CvV − CvL .

(8.132)

Fig. 8.15. The behavior of the function F(η ) in Eq. (8.124) as a function of η

376

8 Irradiation-Induced Voids and Bubbles

Substituting in for CvV and CvL from Eqs. (8.85) and (8.99), respectively, gives: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 2γΩ × 4π RCP ρCPCv0 exp + zv ρN Cv0 exp − Cv0 (8.133) RkT RkT 2γΩ Θ +ρL Cv0 exp − Cv0 exp − √ . RkT 2 mi kT

Approximating exp (x) ∼ x + 1 for small x, in the exponential terms of Eq. (8.133) gives: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 0 × 4π RCP ρCPCv exp RkT

2γΩ 2γΩ Θ 0 + ρL + √ +zvCv ρN , RkT RkT 2 mi kT

(8.134)

and pulling the term Cv0 out into the coefficient yields: R˙ th =

−Dv Ω Cv0 R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 2γΩ A 2γΩ × 4π RCP ρCP exp + zv ρL + √ + zv ρN , RkT RkT RkT 2 mi kT (8.135)

which is the simplified expression for the thermal emission term. This term represents the thermal emission of defects from sinks. It is independent of defect production rate and is strongly temperature-dependent. Note that at very low temperature, R˙ th → 0, because of the terms Dv and Cv0 . ˙ determined from Eq. (8.120), The rate of change in the void radius with time, R, can be used to determine the volumetric swelling rate: dV = 4π R2 R˙ . dt

(8.136)

Void swelling can be represented in terms of the void size distribution as follows. If ρV (R) dR is the number of voids/cm3 with radii between R and R + dR, then the total void number density is:

ρV =

∞ 0

ρV (R) dR ,

(8.137)

the average void size is: R=

1 ρV

∞ 0

RρV (R) dR ,

(8.138)

8.3 Void Growth Equation

377

and the amount of void swelling is defined by the change in volume of the solid: 4 ΔV = π V 3

∞ 0

R3 ρV (R) dR .

(8.139)

If the void distribution is narrow, then we can approximate the integral in Eq. (8.139) with: ΔV 4 3 = π R ρV . V 3

(8.140)

The equations provided in this section allow the determination of the rate of growth of voids in a solid under irradiation, and consequently, the rate of swelling of that solid. The following sections address the effects of various parameters on void growth. 8.3.1 Temperature Dependence Figure 8.16 provides a typical plot of void swelling as a function of temperature. Note that swelling is characterized by a peak at intermediate temperature. This behavior should look familiar from the temperature dependence of RIS since the origin is essentially the same. Low defect mobility limits void growth at low temperature, and the approach of the defect concentration to the thermal equilibrium value, and hence the loss of supersaturation, limits void growth at high temperature. In the preceding analysis of the void growth equation, the two highly temperature sensitive parameters are the vacancy diffusion coefficient Dv and the equilibrium vacancy concentration Cv0 . The temperature dependence of the term R˙ 0 F(η ) is contained in the parameter η , which is controlled by Dv . At low temperatures, swelling is low because vacancies are practically immobile. A low value of Dv makes η large and forces F to become small, resulting in a low value for the term R˙ 0 F(η ). The term R˙ th approaches zero since it is proportional to DvCv0 . Since both F (η ) and R˙ th become small at low temperature, void growth ceases. Under these conditions, the concentration of vacancies builds up and vacancies and interstitials are lost to recombination. At high temperature, the emission of vacancies by voids counterbalances the net vacancy influx driven by irradiation and suppresses swelling. When in the void growth equation η becomes small and F approaches unity, the term R˙ th also increases (but in the negative direction) and dominates at the highest temperatures. Hence a maximum in the growth rate is predicted at intermediate temperature where both thermal emission and mutual recombination are less important and the net flow of vacancies to voids is maximized. Figure 8.17 shows how the components of the void growth rate combine to result in a peak at intermediate temperature. This is found to be true with all metals. Figure 8.18a shows an example of the sharp dependence of void swelling on temperature in an Fe–Cr–Ni alloy irradiated in the BN-350 reactor as a function

378

8 Irradiation-Induced Voids and Bubbles

Fig. 8.16. Swelling in nickel as a function of irradiation temperature for a fluence of 5 × 1019 n/cm2 (after [17])

Fig. 8.17. Construction of the total void swelling rate R˙ from its components R˙ 0 F and R˙ th

of dose and temperature. All the data were for irradiation over a fixed time period, reflecting the variation of dose rates with position in the core. Closed symbols represent samples in which voids were found and open symbols were samples that exhibited no voids. Note that despite the differing doses and dose rates, void nucleation occurs with a very sharp temperature threshold at about 302 – 307 ◦C, illustrating the high sensitivity of void formation to temperature. The gen-

8.3 Void Growth Equation

379

Fig. 8.18. (a) Dosetemperature plot of swelling in a Fe–Cr–Ni alloy irradiated in the BN350 fast reactor showing the sharp temperature threshold for swelling (after [18]). (b) Schematic of the temperature dependence of void density and void size

eral behavior of the void number density and size with temperature is shown in Fig. 8.18b. With increasing temperature, the void density falls logarithmically and the size increases, which is the typical behavior for a process that is dominated by nucleation at low temperatures where the void growth is slow, and by growth at high temperature where the free energy difference driving void growth is small. Figure 8.19 shows images of the microstructure in a baffle bolt used to secure baffle former plates against the baffle in a pressurized water reactor. In this case, the head was closest to the core (received the highest dose), and was exposed to the coolant, hence the lowest temperature. Gamma heating caused the temperature to exceed the coolant temperature (∼ 320 ◦C) along the length of the bolt. While the

380

8 Irradiation-Induced Voids and Bubbles

Fig. 8.19. Swelling in a cold-worked 316 SS baffle bolt in a PWR as a function of position along the bolt length. The bolt head was closest to the core and the temperature distribution is caused by a combination of gamma heating and whether the bolt was exposed to the coolant (courtesy S.M. Bruemmer and Garner FA, PNNL)

doses differ somewhat, the dominant influence of temperature is noted by both the lack of voids in the lowest temperature location (head) and the largest void size at the highest temperature (top shank). 8.3.2 Dose Dependence Understanding how swelling depends on dose is critical in the design and operation of components in radiation environments in which voids have the potential to form and grow. From the discussion in the previous section, the dependence is complicated by the occurrence of the defect production rate, K0 , in the terms R˙ 0 and F(η ). So we will take a different approach in determining the void growth rate dependence on dose, following that of Mansur [5]. Recall the expressions for Cv and Ci given in Eq. (8.119): Di ki2 (η + 1)1/2 − 1 2Kiv Dv kv2 (η + 1)1/2 − 1 , Ci = 2Kiv

Cv =

8.3 Void Growth Equation

381

and for η as given in Eq. (8.117):

η=

4Kiv K0 . Di Dv kv2 ki2

We can write the term in brackets in Eq. (8.119) as: 1/2 4K K iv 0 1+ −1 . (η + 1)1/2 − 1 = Di Dv kv2 ki2 Then, DvCv and DiCi can be written as: Dv Di ki2 zv 4Kiv K0 1/2 DvCv = −1 1+ 2Kiv Di Dv kv2 ki2 Dv Di kv2 zi 4Kiv K0 1/2 DiCi = −1 . 1+ 2Kiv Di Dv kv2 ki2 Neglecting thermal emission, and substituting into Eq. (8.112) gives: 1/2 4K Ω D D K v i iv 0 1+ − 1 (kv2 zv − ki2 zi ) . R˙ = 2RKiv Di Dv kv2 ki2

(8.141)

(8.142)

(8.143)

Substituting for kv2 and ki2 from Eq. (8.104) and considering only coherent precipitates, network dislocations and loops gives: 1/2 Ω D D K 4K v i iv 0 −1 1+ R˙ = 2RKiv Di Dv kv2 ki2 L N CP L N × 4π RCP ρCP zCP . i zv − zv zi + ρL zi zv − zv zi + ρN zi zv − zv zi (8.144) Simplifying Eq. (8.144) for the case of voids and total dislocation density only, we have: 1/2

Ω D D K 4K v i iv 0 (8.145) R˙ = − 1 ρd zdi zv − zdv zi . 1+ 2 2 2RKiv Di Dv k v k i The term zdi zv − zdv zi is the bias of dislocations vs. that for voids and is the determinant of the propensity for a void to grow or shrink. Growth will occur if zdi zv > zdv zi , zd zv and shrinkage will occur if the inequality is in the other or stated as ratios, id > zv zi direction. The presence of other sinks will affect swelling through their inclusion in the terms kv2 and ki2 . The larger the sink strengths, the lower will be the void growth rate due to the loss of defects to those sinks.

382

8 Irradiation-Induced Voids and Bubbles

The limiting behaviors of Eq. (8.145) are the cases in which recombination dom4Kiv K0 inates

1 (loss of defects to recombination is much larger than that lost Di Dv kv2 ki2 4Kiv K0 to sinks) and loss to sinks dominates 1 [5]. Assuming that the only Di Dv kv2 ki2 sinks besides voids are network dislocations, we have: 1/2 1/2 Ω Di Dv K0 1/2 Qi Qv zNi zv − zNv zi ˙ R= : recombination dominant R zNi zNv Kiv (1 + Qv)1/2 (1 + Qi)1/2 (8.146) N Ω K0 Qi Qv R˙ = z zv − zNv zi : sink dominant , RρN (1 + Qv)(1 + Qi ) i (8.147) where: Qi,v =

zNi,v ρN 4π Rρvzi,v

(8.148)

is the ratio of dislocation sink strength to void sink strength. Note that the growth 1/2 rate is dependent on K0 when recombination is dominant, Eq. (8.146). However, when sinks are dominant, Eq. (8.147) shows that the growth rate is proportional to K0 . Multiplying Eq. (8.147) by 4π R2ρV and given that Ω = 1/N0 , the site density, gives the volume swelling rate: zi − zv Q d(ΔV /V ) = K0 . (8.149) dt zv (1 + Q)2 This is the same expression that can be obtained from Eq. (8.122) by neglecting the effect of coherent precipitates. For Q = 1 and zi − zv = 0.01, we have: ΔV ∼ % = 1/4 × (dose in dpa) . V

(8.150)

Garner [19] has shown that over a wide dose range, the steady state swelling rate is of the order of ∼ 1%/dpa (Fig. 8.20). The linear dependence is consistent with a sink-dominated process, but the magnitude of the coefficient is a factor of four greater than that predicted by Eq. (8.150). The discrepancy is likely due to the effect of clusters that is not accounted for in the rate theory model. A closer look at the behavior of vacancies and interstitials in the cascade shows that the fraction of vacancies and interstitials that form clusters is larger than has been accounted for thus far. Vacancy clusters form near the cascade core and interstitial clusters form near the cascade periphery. Mobile interstitial clusters can reach sinks by migration of the cluster as a whole. Vacancies emitted by vacancy clusters by thermal emission are also free to reach sinks. Since the fraction of interstitials and vacancies in clusters is not the same, nor is their thermal stability, the difference between vacancy and interstitial clusters results in a difference in the effective production rates of vacancies

8.3 Void Growth Equation

383

Fig. 8.20. (a) Early development of 1%/dpa swelling rates in aged OKH16N15M3B steel during irradiation in the BOR-60 reactor at 400 – 550 ◦C (after [20]). (b) Variations in swelling at 540 ◦C in EBR-II for two nominally similar heats of 316 stainless steel as a function of starting condition (after [21])

compared to that of interstitials, termed the production bias, and can influence void swelling. The net result is that the sink strength of the clusters is much greater than that of the measurable dislocation loops, resulting in a much greater driving force for void swelling than is accounted for by the rate equation formulation. This is one of the reasons that the observed steady state swelling dependence on dose is greater than that predicted by the rate equation formulation.

384

8 Irradiation-Induced Voids and Bubbles

8.3.3 Role of Dislocations as Biased Sinks The dislocation structure of an alloy can exert a profound effect on the swelling behavior. Equation (8.122) demonstrates that both a biased sink (e.g., dislocations) and a neutral sink are necessary for void growth. If the bias was removed, zi = zv , then R˙ 0 = 0 and swelling will not occur as defects will flow equally to each sink. The Q-dependence of R˙ 0 is shown in Fig. 8.21. Note that R˙ 0 is a maximum at Q = 1, or when the flow of vacancies to voids and dislocations is equal. The regime Q < 1 is representative of the low dose regime in which both R and ρV are small, so vacancy loss to the existing dislocation network dominates. This is why cold-worked alloys swell less. When Q ∼ 1, then the flow of vacancies to voids and dislocations is approximately equal. This is the regime where bias exerts its greatest influence. If the flow of vacancies and interstitials to sinks is equal, and more interstitials go to dislocations, then more vacancies must flow to voids. At Q ∼ 1, the flows are equal so the bias is most effective in promoting void growth. When Q > 1, defect flow to voids dominates the loss terms and since few defects flow to dislocations, the bias is not very effective in creating an imbalance in point defect fluxes, so the flow of vacancies and interstitials to voids is similar in magnitude and void growthslows orceases. Although dislocations exhibit βd ≥ 1 , in a cold-worked material, the disloa slight preference for interstitials βV cations provide so many sinks for vacancies that the effect of a vacancy supersaturation is essentially multiplied, resulting in low void nucleation and growth rates. By the same mechanism, grain boundaries provide unbiased sinks for point defects and will keep the vacancy supersaturation too low for growth provided the grain boundary area is large enough (i.e., very small grains). Figure 8.22 shows a plot of swelling rate vs. the sink strength ratio, Q for several austenitic stainless steels and verifies that indeed, the dependence shown in Fig. 8.21 is obeyed in practice. The effect of cold-work on swelling in reactor exposures is shown in Fig. 8.23. Figure 8.23a shows the effect of cold-work on swelling in 316 stainless steel ir-

Fig. 8.21. Dependence of swelling on the dislocation/void sink strength ratio, Q in Eq. (8.149)

8.3 Void Growth Equation

385

Fig. 8.22. Experimentally observed swelling rates as a function of Q for austenitic stainless steels (after [5])

radiated in EBR-II at 650 ◦C to levels of 33 and 50 dpa. Note that for both cases, the amount of swelling decreases with increasing cold-work. Figure 8.23b shows that cold-work affects the temperature dependence of swelling by suppressing the magnitude of the swelling peak with increasing levels of cold-work. The data are taken from a stainless steel irradiated to doses of 20 – 61 dpa in the RAPSODIE reactor. Figure 8.23c shows the effect of cold-work on the dose dependence of swelling in 304 stainless steel, and that increasing cold-work decreases the amount of swelling, but at reduced rates as the amount of cold-work increases. Note also that these data show that the primary effect of cold-work is to extend the transient swelling regime, rather than to alter the steady state swelling rate. 8.3.4 Dose Rate Dependence The location of the peak swelling temperature depends on the dose rate, sink strength and the predominant mode of defect loss. When the dose rate increases, more point defects are created, but their migration velocities are unchanged. To remove defects at the higher rate at steady state requires point defect concentrations to be higher, resulting in greater recombination and a reduction in the net absorption of vacancies by voids, and hence, a reduction in the void growth rate. As a result,

386

8 Irradiation-Induced Voids and Bubbles

Fig. 8.23. (a) Effect of cold-work level on the swelling of 316 stainless steel irradiated at 650 ◦C in EBR-II to 33 and 50 dpa (after [22]). (b) Dependence of swelling on cold-work for various temperatures for 316 stainless steel irradiated in the RAPSODIE reactor to doses of 20 – 71 dpa (after [23]). (c) Effect of cold-work on swelling in 304 stainless steel at 450 ◦C in EBR-II (after [24])

8.3 Void Growth Equation

387

the bell-shaped swelling curve is displaced to higher temperatures with increasing dose rate. Figure 8.24 is a plot of the temperature dependence of the term F(η ) in Eq. (8.125), and illustrates the shift of the swelling peak with dose rate, K0 . Alternatively, at a given temperature, the void growth rate decreases for increasing dose rate. At temperatures where thermal emission is non-negligible, the void growth rate is a complicated function of dose rate. Nevertheless, the experimental data substantiate the effect of dose rate on swelling. Figure 8.25 shows swelling in annealed and

Fig. 8.24. Variation of the function F(η ) in Eq. (8.124) with temperature, illustrating the shift of the peak with dose rate, K0 . Parameters used to construct the curves are as follows: ρd = 109 cm−2 , Efv = 1.6 eV, zi − zv = 0.01, zv = 1, 4π RρV = 10−11 cm−2 , Dv = exp(−1.4 eV/kT ) cm2 s−1 (after [15])

Fig. 8.25. (a) Effect of displacement rate on swelling of annealed 316 stainless steel in the RAPSODIE reactor fuel pin cladding at 562 ◦C. (b) Swelling in cold-worked 316 stainless steel in the PHENIX reactor fuel pin cladding at 590 – 610 ◦C (after [25] and [26])

388

8 Irradiation-Induced Voids and Bubbles

cold-worked 316 stainless steel at temperatures between 562 and 610 ◦C over a range of dose rates. Note that increasing dose rate has the effect of reducing the swelling rate at a given dose, but that at steady state, all data have a similar slope, indicating that the primary effect of dose rate is on the duration of the swelling transition period. If we move up the temperature scale, we can restore the same relative ratio of recombination rate to absorption rate at sinks. In fact, by requiring that this ratio be invariant, we can obtain a relationship between temperature and dose rate, termed the temperature shift. 8.3.5 Irradiation Variable Shifts The concept of variable shifts was developed to provide a better understanding of the relationship between variables in swelling [16]. The idea is that when one irradiation variable is changed, a shift in other variables can be determined that will preserve a physical quantity describing the behavior of defects during irradiation. There are two such quantities that pertain to the limiting case where recombination dominates defect loss. The number of defects per unit volume that have recombined up to a time τ is: NR = Kiv

τ 0

CiCv dt .

(8.151)

When the solid is at steady state and defect concentrations are controlled by recombination, Eq. (8.116) give:

K0 zi Di 1/2 Kiv zv Dv K0 zv Dv 1/2 Ci = , Kiv zi Di Cv =

(8.152)

and substituting into Eq. (8.151) yields: NR = K0 τ .

(8.153)

The number of defects lost to sinks per unit volume up to a time τ is: NSj =

τ 0

K jC j dt ,

(8.154)

where the subscript j denotes the defect type. Substituting Eq. (8.152) into Eq. (8.154) gives for vacancies: NSv =

KV (K0 Kiv )1/2

zi Di zv Dv

1/2

Φ,

where Φ is the dose, and the expression for interstitials is identical.

(8.155)

8.3 Void Growth Equation

389

These definitions can be used to determine relationships between any two of the three variables: temperature, dose and dose rate, taking the third to be constant. For example, in the steady state recombination-dominated regime, we may require Ns to be equal for dose 1 and dose rate 1 to that for dose 2 and dose rate 2 at a fixed temperature: KV (K01 Kiv )1/2

zi Di zv Dv

1/2

KV Φ1 = (K02 Kiv )1/2

zi Di zv Dv

1/2

Φ2 ,

and canceling terms in the equality gives:

Φ2 = Φ1

K01 K02

1/2 .

(8.156)

For a given change in dose rate, the shift in temperature required at constant dose to keep Ns invariant is determined by equating the same terms, but with fixed dose, resulting in:

Dv K0

1/2

=

1

Dv K0

1/2 ,

(8.157)

2

v /kT ): or substituting in for Dv from Eq. (4.54), Dv = D0 exp(−Em K02 kT12 ln v Em K 01 . T2 − T1 = K02 kT1 1 − v ln Em K01

(8.158)

For a change in dose, the shift in temperature required to maintain Ns invariant at fixed dose rate is: 1/2

1/2

(Dv Φ )1 = (Dv Φ )2 , and substituting in for Dv :

v E Φ2 1 1 = exp m − , Φ1 2k T2 T1

(8.159)

(8.160)

and re-arranging gives: −2kT12 Φ2 ln v Em Φ1 T2 − T1 = . 2kT1 Φ2 1 + v ln Em Φ1

(8.161)

There is another important temperature shift that, instead of requiring that Ns be invariant, requires the net flux of vacancies over interstitials to a particular type

390

8 Irradiation-Induced Voids and Bubbles

of sink (voids in this case) to be invariant, where the net flux is relevant to void swelling. The temperature shift derived in this way for the recombination-dominated regime to keep swelling rate (NR ) invariant is [16]: kT12 v Em + 2Efv

K02 K01 T2 − T1 = . K02 kT1 1− v ln Em + 2Efv K01 ln

(8.162)

where Efv is the vacancy formation energy. The various variable shifts described in this section are shown in the following figures. Figure 8.26 shows the relationship between dose vs. dose rate dependence at a reference temperature of 200 ◦C for the case of Ns invariant, Eq. (8.156). Figure 8.27 shows the temperature shift as a function of dose rate at constant dose for three values of vacancy migration energy for Ns invariant, Eq. (8.158), and Fig. 8.28 shows the same relationship for the constant dose rate case, Eq. (8.161). Figure 8.29 shows the temperature shift as a function of dose for constant dose rate to keep the swelling rate, NR invariant, Eq. (8.162). Figure 8.30 shows that the temperature shift concept works well in describing the shift in the peak in the swelling vs. temperature curve in nickel over more than five orders of magnitude in the dose rate as given by Eq. (8.162).

Fig. 8.26. Number of interstitials absorbed at sinks as a function of dose at 200 ◦C for different dose rates (after [27])

8.3 Void Growth Equation

391

Fig. 8.27. Temperature shift from the reference 200 ◦C required at constant dose in order to maintain the same point defect absorption at sinks as a function of dose rate, normalized to initial dose rate. Results are shown for three different vacancy migration energies (after [8.27])

Fig. 8.28. Temperature shift from the reference 200 ◦C required at constant dose rate in order to maintain the same point defect absorption at sinks as a function of dose, normalized to initial dose. Results are shown for three different vacancy migration energies (after [8.27])

392

8 Irradiation-Induced Voids and Bubbles

Fig. 8.29. Temperature shift from the reference 200 ◦C required at constant dose in order to maintain swelling invariance as a function of dose rate, normalized to initial dose rate. Results are shown for three different vacancy migration energies and a formation energy of 1.5 eV

Fig. 8.30. Temperature shift of peak swelling as a function of dose rate. Points are experimental data and the line is from theory (after [5])

8.3 Void Growth Equation

393

8.3.6 Stress Dependence Equation (8.125) shows that the void growth rate consists of two components. R˙ th is the thermal emission terms and hence is the only part affected by the state of stress or internal gas pressure. Consequently, the internal gas pressure and stress begin to affect the growth rate only when R˙ th becomes significant, i.e., for temperatures greater than the peak swelling temperature. When the solid is under a hydrostatic stress and when voids contain gas that exerts a pressure on the void surface, the equilibrium vacancy concentration at voids and dislocations will be different from that in the stress-free, gas-free state. Brailsford and Bullough showed that the pressure, but not the external stress, will affect the concentration of vacancies in equilibrium with the void. Hence, the force balance for the void surface of a bubble in mechanical equilibrium, Eq. (8.82), becomes: 2γ , (8.163) R where σ is the hydrostatic stress and p is the gas pressure in the void. (In the case of a non-equilibrium bubble, the appropriate stress is the radial component of the stress tensor, σr .) The vacancy concentration at the surface of the void, given by Eq. (8.85) in the gas-free case, becomes:

Ω 2γ V 0 Cv = Cv exp − p− . (8.164) kT R

σ = p−

Similarly, the equilibrium vacancy concentration adjacent to the network dislocations becomes:

σΩ CvN = Cv0 exp − . (8.165) kT Repeating the solution to the void growth equation using the equilibrium vacancy concentration at the void surface given by Eq. (8.164) and the equilibrium vacancy concentration at the network dislocations given by Eq. (8.165) revises the thermal emission term, Rth in Eq. (8.135) (with ρCP = ρL = 0) as follows: 2γ 0 2 DvCv Ω zv ρd σ + p − R R˙ th = . (8.166) RkT (zv ρd + 4π RρV) Note that shrinkage due to thermal emission becomes instead, stress-enhanced growth when the sum of the external stress and gas pressure exceed the stress due to surface tension: 2γ . (8.167) σ+p> R Note that for a stressed solid containing no gas, stress-enhanced growth will occur 2γ when σ > . For a void containing x gas atoms, Eq. (8.167) becomes: R 3xkT 2γ − σ= . (8.168) R 4 π R3

394

8 Irradiation-Induced Voids and Bubbles

The void radius at which Rcr =

9xkT 8πγ

dσ = 0 is called the critical void radius and is given by: dR

1/2 ,

(8.169)

and substituting into Eq. (8.165) gives the stress at the critical void size, which is the critical stress for unlimited void growth: 4γ 8πγ 1/2 σcr = . (8.170) 3 9xkT The effect of stress on void growth in steel is given in Fig. 8.31. Note that there is little effect of stress out to high dose when the stress is low. But when stress is increased, the swelling increases rapidly at relatively lower doses. Figure 8.32 also accounts for the presence of helium in the growth of voids under stress. However, this formulation predicts that the void growth rate is proportional to stress, which is counter to the 1%/dpa observations. Also, as shown in Fig. 8.32, the effect of stress is only significant at very high temperatures. Experimental data have since shown that the prime role of stress is on shortening the transient swelling regime, rather than increasing the swelling rate in the steady state regime. Figure 8.33 shows the effect of stress on swelling in modified 316 stainless steel alloys irradiated in the PHENIX reactor. Note that with increasing stress, the swelling rate (slope) approaches a constant value at lower doses. Stress can also affect the stability of void nuclei, which would explain the observation of more rapid nucleation.

Fig. 8.31. Stress-enhanced swelling for various stress levels and temperatures as a function of fluence (after [28])

8.3 Void Growth Equation

395

Fig. 8.32. Temperature dependence of stress-enhanced void growth in steel. The solid curves apply to a dislocation density of 109 cm−2 . And a helium production rate of 10−6 appm/s (after [29]) Fig. 8.33. Effect of stress on swelling of two modified 316 stainless steels irradiated in the form of pressurized tubes in the PHENIX reactor (after [30])

In the development of the nucleation rate of voids, the nucleation current and number density of voids of size n was described by Eqs. (8.18) and (8.19), respectively, for the case of vacancy condensation excluding interstitials: −ΔG0n −ΔG0n Jn = Z β N0 exp , and ρ 0 (n) = N0 exp . kT kT

396

8 Irradiation-Induced Voids and Bubbles

with the free energy of formation of void of size n given by Eq. (8.17): ΔG0n = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 . Accounting for the application of an external hydrostatic stress, σh , gives: ΔG0n (σh ) = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 − nσhΩ ,

(8.171)

ΔG0n (σh ) = ΔG0n (0) + nσhΩ .

(8.172)

and

Note that the effect of gas pressure, p, in the void can also be accounted for by addition of a term, npΩ . When interstitials are present, the free energy is given by Eq. (8.33): ΔGn

δ G0j βi ( j + 1) + exp , = kT ∑ ln βv ( j) kT j=0 n−1

where δ G0j /kT is the increment in free energy of a void in going from j vacancies to j + 1 vacancies if no interstitials are present. By assuming that stress affects only the free energy barrier (and not the critical nucleus size), and that the stress contribution of the energy per atom is not dependent on the number of atoms in the cluster, then we can approximate the free energy in Eq. (8.33) in a manner similar to that done in Eq. (8.172) [31]: ΔGn (σh ) = ΔGn (0) + nσhΩ .

(8.173)

Then, from Eq. (8.35), the ratio of stressed to unstressed steady state nucleation rates in a homogeneous, co-precipitation environment is: Jn (σh ) exp[−(ΔGn − nσhΩ )/kT ] = . Jn (0) exp[−ΔGn /kT ]

(8.174)

Using Eqs. (8.22) and (8.23) to write the ratio of nucleation currents in terms of the ratio of void number densities in the stressed and unstressed state gives: Jn (σh ) Z (σh )βn (σh )ρn (σh ) Z (σh )βn (σh ) exp[−(ΔGn (σh ))] = = , Jn (0) Z (0)βn (0)ρn (0) Z (0)βn (0) exp[−Δ Gn (0)]

(8.175)

and provided that neither the arrival rate ratio, βn (σh )/βn (0), nor Z is sensitive to the stress level [32], then Eq. (8.175) becomes:

ρn (σh ) ≈ exp(nσn Ω /kT ) . ρn (0)

(8.176)

8.3 Void Growth Equation

397

Fig. 8.34. Variation of the void nucleation rate and the void number density as a function of stress and temperature, as described by Eq. (8.176)

Example 8.1. Effect of stress on void density Assuming an external stress of 100 MPa and a void cluster size of ∼ 15 at a temperature of 450 ◦C, Eq. (8.176) gives an increase in the void number density by a factor of ∼ 6. However, for a stress of 200 MPa, the increase is 34 and for 300 MPa, the factor becomes ∼ 200. Since both stress and temperature appear in the exponent, the factor rises rapidly with an increase in stress and with a decrease in temperature (Fig. 8.34). Referring back to Fig. 8.33, the decreasing time to reach the steady state swelling rate as stress is increased, is explainable by stress-enhanced nucleation, which will be more important at lower temperatures, contrary to the effect of stress on the steady state swelling rate.

8.3.7 Effect of RIS Recall from Chap. 6, Sect. 6.4, that RIS (radiation-induced segregation) of the major elements occurs at sinks, which can include voids. The result is a coated void in which the void develops a shell of composition that is different from that in the matrix. As we have seen, for austenitic stainless steels, the void coating is enriched in nickel and depleted in chromium relative to the matrix. A primary effect of the composition change is a change in diffusion coefficient leading to a change in the void capture efficiency. The capture efficiency for the vacancy in the shell is [16, 33]: zV v (rV ) =

1 + δ /rV , 1 + Dvδ /DSv rV

(8.177)

where δ is the thickness of the shell and DSv is the vacancy diffusion coefficient in the shell. Recall that an expression for the composition dependence of Dv in the shell, DSv was determined in Sect. 6.4 of Chap. 6. Using the expression for the capture efficiency in the void growth equations results in a reduction in void growth if DSv < Dv and DSi ∼ Di . A more important effect of the coating is the elastic interaction between a point defect and a void surrounded with a coating that has different elastic constants than

398

8 Irradiation-Induced Voids and Bubbles

the matrix. The result is a change in capture efficiency of the void for defects. The capture efficiency due to a difference in elastic constants is given as:

rV rV Di,v −1 (r ) = + , (8.178) zV i,v V rc (rc + δ )2 wi,v where rc is the void plus coating radius and the transfer velocity, wi,v is: wi,v =

∗ /kT ) Di,v exp(−Ei,v , a

(8.179)

where a is the lattice parameter and E ∗ is the repulsive interaction energy at its largest positive value. The sign of E ∗ is positive (repulsion) if the matrix of the shell is stiffer than that of the matrix. Since E ∗ is proportional to the square of the point defect relaxation volume, the sink efficiency is much smaller for the interstitial than for the vacancy due to the larger repulsion for the interstitial. So the stiffer shell results in a repulsion that is greater for the interstitial than for the vacancy, making void nucleation and growth more rapid in the case of a coated void (Fig. 8.35). A change in the shear modulus or lattice parameter in the shell can also alter the preference of the void for vacancies and interstitials [34] by creating a barrier to defect diffusion through the shell due to a change in the strain energy. When segregation leads to a shell with a shear modulus or lattice parameter only slightly higher than in the surrounding matrix, the void becomes a highly preferential sink for vacancies and swelling is increased. Conversely, a reduction in the shear modulus and

Fig. 8.35. Capture efficiencies for point defects diffusion to a void and a coated void as a function of void radius, rV . The void prefers interstitials, especially at small void sizes. The preference is reversed for the coated void (after [16])

8.3 Void Growth Equation

399

Fig. 8.36. Capture ratio z0i /z0v for coated voids with a shell thickness of two atomic layers and zero surface stress (after [34])

lattice parameter should result in reduced void swelling. Figure 8.36 shows the effect of the shear modulus (1 − μbulk/μshell ) on the interstitial/vacancy capture ratio. For small voids, a few percent change in the shear modulus can result in orders of magnitude change in the capture ratio. Allen et al. [35] compared the swelling and RIS behavior of a range of alloys with different nickel content. Calculation of the lattice parameter for the void shell composition shows that the swelling behavior can be explained by a decrease in lattice parameter at the void surface (Fig. 8.37). In fact, segregation leads to a smaller lattice parameter with a lower shear modulus, and the softer shell reduces void swelling. 8.3.8 Effect of Production Bias Our formulation of swelling was developed under the assumption that only single vacancies and interstitials contribute to the growth or shrinkage of the void. If we wish to include the effect of interstitial clustering and mobility in the damage cascade in this picture, then the most straightforward way to do this is to return to clustering theory and describe the evolution of the void embryo with consideration of interstitial clusters. Numerical solution to the Fokker–Planck equation will yield the void size distribution as a function of time or dose. (An example of the results of such an analysis was presented in Chap. 7 for interstitial loops.) However, numerical solutions are not of much value in understanding the process and the importance of various parameters in the evolution of the void population. Another approach is to consider the effect of the asymmetric production of vacancies and interstitials (production bias) due to differences in the fractions that agglomerate into clusters and

400

8 Irradiation-Induced Voids and Bubbles

Fig. 8.37. Decrease in swelling as a function of changing lattice parameter. Swelling decreases with decreasing lattice parameter, which is caused by RIS at the void surface (after [35])

differences in the thermal stability and mobility of vacancy and interstitial clusters. So we will consider the case when the interaction of the glissile loops with vacancy and SIA loops is negligibly small, in which case, we can develop an analytical expression for swelling which still captures the effect of clustering [36, 37]. Under cascade conditions where clustering is expected to occur, we modify the vacancy and interstitial steady state point defect balance equations by adding in glissile SIA clusters with the following result: 2 vc 2 (1 − εig)K0eff = DiCi (zi kv2 + zdi ρd ) + Kiv DiCiCv + zic v DvCv kni + zi DiCi knv

(8.180) K0eff

2 vc 2 = DvCv (zv kv2 + zdv ρd ) + Kiv DiCiCv + zic v DvCv kni + zi DiCi knv

(8.181)

εig K0eff /xg

= DgCg kg2 ,

(8.182)

where K0eff = (1 − εT )K0 is the effective Frenkel pair generation rate obtained from the NRT rate by accounting for the fraction of Frenkel pairs, εT , recombining dur2 vc 2 ing cascade cooling, and zic v kni and zi knv are the sink strengths of sessile SIA clusters (ic) and vacancy clusters (vc) for the absorption of vacancies (v) and SIA clusg ters (i), respectivly. The quantity, g refers to glissile clusters, εi is the fraction of SIAs in glissile clusters and xg is the mean cluster size. The term kg2 is the total sink strength for the 1D diffusing SIA clusters:

8.3 Void Growth Equation

kg =

1/2 2 πρ dabs + + π R2 ρ V , 4 l(2Rg − l)

401

(8.183)

where dabs is the effective diameter of dislocations for absorbing glissile SIA cluster, Rg and l are the grain radius and distance from the cluster to the grain boundary, respectively. Under cascade damage conditions that allow for intracascade clustering of SIAs and also cluster removal by 1D diffusion of glissile SIA cluster, the void swelling rate is determined by the fluxes of point defects and glissile SIA clusters to voids. Equation (8.110) then becomes: d(ΔV /V ) = (DvCv zv − DiCi zi )kv2 − DgCg xg kg π R2 ρV . (8.184) dt The second term in Eq. (8.184) comes from Eq. (8.182). Under cascade damage conditions, the difference in the point defect fluxes to dislocations due to dislocation bias as well as the recombination and effect of cluster terms in Eqs. (8.180) and (8.181) cause only small perturbations in the swelling rate at steady state. Neglecting recombination and defect cluster terms in Eqs. (8.180) and (8.181), then Eq. (8.184) becomes:

zv kv2 π R2 ρ V d(ΔV /V ) g eff = K0 εi − dt zv kv2 + zdv ρd kg 2 d zv kv zv ρd g +(1 − εi )pl , (8.185) (zi kv2 + zdi ρd )(zv kv2 + zdv ρd ) where pl = (zdi /zdv − zi /zv ) ≈ (zdi /zdv − 1), and zv + zi = 1. The swelling rate is proportional to the effective generation rate and the damage efficiency. The first term in square brackets in Eq. (8.185) is the contribution of the production bias to swelling and is proportional to the glissile cluster fraction explicitly. The second term is due to conventional dislocation bias controlled by single point defects, as is evident by its (1 − εig ) proportionality. For the limiting case of g single Frenkel pair production, where no clusters are formed, εi = 0, the first term vanishes and the swelling rate is driven by single point defect absorption controlled by dislocation bias. The resulting expression is the same as that given in Eq. (8.122) g (neglecting coherent precipitates). Conversely, when εi is close to 1.0, the conventional dislocation bias contribution is small compared to that due to production bias. When both single SIAs and SIA clusters exhibit 3D diffusion, the swelling rate follows an expression analogous to that determined for the single defect, dislocation bias case, Eq. (8.122); however, an SIA cluster term is now included that is analogous to that for single SIAs and can be written as:

g 2 d (1 − εi )p εig pcl d(ΔV /V ) eff zv kv zv ρd = K0 + , (8.186) dt (zv kv2 + zdv ρd ) zcl kv2 + zdv ρd (zv kv2 + zdv ρd ) where pcl = (zdcl /zdv − zcl /zv ) is the bias factor for SIA clusters. Equation (8.186) results in a positive swelling rate for 3D cluster reaction kinetics for any microstructure, similar that in the single defect, dislocation bias formulation, meaning that saturation of swelling will not occur.

402

8 Irradiation-Induced Voids and Bubbles

A permanently positive swelling rate is not physically plausible as swelling is known to saturate at high doses and high values of swelling. In fact, the general behavior of the solution of the Fokker–Planck equation is a gradual broadening of the size distribution until steady state is reached as cascade damage limits further growth of interstitial clusters. According to Eq. (8.185), the swelling rate decreases with increasing void size because of their increasing efficiency for capturing glissile SIA clusters, and the swelling rate will drop to zero when a maximum void size, Rmax , is reached. Under this condition, and if the void density remains constant, the swelling rate saturates when the swelling reaches some value, (ΔV /V )max . In the case where production bias dominates, the saturation void size and saturation swelling become, from Eq. (8.185): Rmax = π dabs /zdv , (ΔV /V )max =

4π max 3 (R ) ρV . 3

(8.187)

Note that neither Rmax nor (ΔV /V )max depend on cascade parameters εi or εT , and Rmax is even independent of the void number density, ρV . If cluster formation is ignored in Eq. (8.185), then the swelling rate does not vanish. The saturation of swelling is an intrinsic property of production bias under cascade damage conditions. As presented in the description of clusters using the Fokker–Planck formulation (Sect. 7.6), it was noted that the cluster size distribution is broadened by the parameter D and shifted by the parameter F. Thus, with increasing dose, the solution to the Fokker–Planck equation describes the broadening of the void size distribution and the increase in the mean void size of the distribution with dose. This general behavior can be compared with experimental swelling results for Fe–Cr–Ni irradiated at 650 ◦C. Figure 8.38 shows that the mean size of the distribution increases from about 11 nm at 9 dpa to over 50 nm by 80 dpa with a corresponding broadening of the distribution. Since swelling is mainly sensitive to the shift of the mean size of the distribution, linear swelling (ΔV /V α dose) is obtained when the growth rate is large compared to the diffusional broadening, in which case the swelling rate is then given by the drift force alone. g

8.3.9 Void Lattices Voids have also been found to organize themselves in periodic arrays, or lattices in a metal under irradiation. Figure 8.39a shows a void lattice in bcc Nb following irradiation with 8.5 MeV Ta+ to a dose of 300 dpa at 800 ◦C, and Fig. 8.39b shows one in Mo irradiated with 2 MeV N+ ions to a dose of 100 dpa at 870 ◦C. The lattices are much easier to form in bcc metals than in fcc metals, though lattices have been observed in Ni, Al and stainless steel. Void lattices are a form of self-organization that occurs as responses of complex systems to external stimuli. It is believed that self-organization results from the collective interaction between system components under external forces that drive the system far from equilibrium. In irradiated solids, the void patterns are believed to be linked to the collective action of the point defects on the lattice structure.

8.3 Void Growth Equation

403

Fig. 8.38. Experimentally measured void size distribution in a Fe–Cr–Ni alloy irradiated at 650 ◦C (after [36])

A full understanding of the formation of void lattices is still lacking, but the theory is able to account for many of the parametric effects in lattice formation. Kinetic rate theory and the determination of an instability threshold can explain many of the observations to date. In general, ordered defect structures form when the following general conditions are satisfied [39]: 1. Agglomeration of vacancies into clusters during the collisional phase of cascade cooling 2. A bias for dislocations towards preferential absorption of interstitials over vacancies 3. An asymmetry in the production and diffusion of mobile point defects (production bias) 4. Some degree of anisotropy during the evolution of clustered defects. This could either be triggered by diffusional anisotropies of point defects, or by anisotropic elastic interaction between defect clusters during the latter stages of their evolution. The occurrence of void lattice formation under cascade damage conditions (neutron or ion irradiation) and its absence under single Frenkel pair production (electron irradiation) is strong evidence for a key role of the 1D motion of thermally stable SIA clusters directly produced in cascades. In fact, it has been shown that when there is anisotropic transport of self-interstitial atoms by the crowdion mechanism (i.e., transport in which some crystal directions are preferred over others), voids occupying spatial positions that form a regular lattice grow faster, on average, than the randomly distributed voids [40]. However, for the void lattice to

404

8 Irradiation-Induced Voids and Bubbles Fig. 8.39. Void lattice in (a) Nb irradiated with 8.5 MeV Ta+ at 800 ◦C to 300 dpa, and helium bubble lattice in (b) Mo irradiated with 2 MeV N+ ions to a dose of 100 dpa at 870 ◦C (after [39])

form, randomly distributed voids have to disappear. This can occur through stochastic void coarsening. Since void evolution in this case is sensitive to the spatial variations in the void growth rate, even a small fraction of interstitials moving as crowdions can significantly affect the spatial behavior of the void ensemble, resulting in the dissolution of randomly distributed voids with lower growth rates by stochastic fluctuations, and the nucleation and growth of voids forming a regular lattice. 8.3.10 Effect of Microstructure and Composition The alloy microstructure can exert significant effects on void nucleation and growth. Microstructure features such as composition, solute addition and precipitate structure are among the most important in influencing void behavior.

8.3 Void Growth Equation

405

Major Element Composition In simple Fe–Cr–Ni austenitic alloys, swelling drops dramatically with increasing nickel content, reaching a minimum at about 50 at%. Figure 8.40 shows that the swelling dependence of nickel holds for various particle irradiations. The effect of Ni content on swelling is primarily due to the change in incubation dose as shown in Fig. 8.41. In fact, the data in Fig. 8.42 shows that at steady state, the swelling rate is the same over a wide range of nickel content. Chromium content also affects swelling of austenitic alloys. Figure 8.43 shows that increasing chromium over the range 15 to 30% results in greater swelling. Less data is available on the systematic effect of Cr than for Ni, but the available data suggests swelling increases monotonically with Cr content. Swelling is much less of a problem in ferritic alloys, but reaches a maximum with a chromium content of about 15 at%. Figure 8.44 summarizes the effect of Ni and Cr on swelling in Fe–Cr–Ni alloys at 675 ◦C. Solute Additions Void swelling should be inhibited by additions of minor elements that bind either vacancies or interstitials with sufficient strength to reduce the effective mobility, thus preventing defects from reaching sinks and promoting recombination. The effect of solutes on the point defect balance equations was presented in Chap. 6, Sect. 6.4. The effect of solute addition on void swelling behavior can be determined by solving Eq. (6.57) through Eq. (6.61) and the nucleation rate, Eq. (8.35), and the void

Fig. 8.40. The effect of bulk nickel concentration on swelling resulting from irradiation with different particles: neutrons, nickel ions and protons (after [35])

406

8 Irradiation-Induced Voids and Bubbles

Fig. 8.41. The influence of temperature and nickel content on swelling of ternary Fe–15Cr– xNi alloys in EBR-II (after [41])

swelling rate, Eq. (8.112). Results of numerical methods solution [42] show that with increasing values of binding energy, the activation energy for void nucleation increases (Fig. 8.45). The void swelling rate decreases with increasing binding energy as shown in Fig. 8.46. The net effect of solute addition on void swelling is shown in Fig. 8.47 which indicates that for increased solute concentration and binding energy, void swelling decreases. Data on the role of solutes in swelling is in general agreement with the model. Figure 8.48 shows that Si and P strongly influence the swelling of austenitic stainless steels. In fact, Si is a fast diffuser and is known to alter the ratio of diffusivities of the solvent atoms. As shown in Fig. 8.49, the effect of P on swelling is indeed in extending the incubation period to larger doses. Oversize solutes such as Hf have a similar effect in suppressing the nucleation of voids in stainless steels irradiated at ∼ 300 ◦C. While other factors are important, Fig. 8.50 shows that the addition of ∼ 1 wt% Hf to 316 stainless steel results in the suppression of void formation during Ni++ ion irradiation at 500 ◦C through a dose of 50 dpa, compared to an incubation dose of only 2 dpa for the reference 316 stainless steel alloy. Precipitates Precipitates can act as recombination sites for vacancy–interstitial annihilation to reduce void swelling. Precipitates can also inhibit dislocation climb necessary for dislocations to act as a preferential sink for interstitials and hence, retard void growth.

8.3 Void Growth Equation

407

Fig. 8.42. Swelling of Fe–15Cr–Ni ternary alloys in EBR-II at temperatures between 400 and 510 ◦C for nickel levels between 12.1 and 24.4 wt% (after [41])

In fact, precipitates can affect cavity growth in three ways [46]. The first is a direct effect in which voids that are attached to precipitates can undergo large growth rates because the precipitate acts as a collector of point defects. Precipitates can indirectly affect void growth by changing the overall sink strength of the solid, or by changing the characteristics of the matrix. As discussed in Sect. 5.8, the coherent precipitate is considered to be a site where constrained recombination of defects occurs due to the distribution of saturable traps that acquire a steady state occupation probability as a result of a balance between defect capture, defect thermal release and extrinsic recombination with the antidefect. However, incoherent precipitates accept any excess point defect flux that happens to impinge on it. These precipitates can accumulate defects and may act as sites for rapid transport of defects, similar to grain boundaries. In fact, they can serve as sites for the collection of defects which are then channeled to voids.

408

8 Irradiation-Induced Voids and Bubbles

Fig. 8.43. Effect of chromium content on swelling in Fe–Cr–Ni alloys following 5 MeV Ni+ ion irradiations to a dose of 140 dpa (after [19])

Fig. 8.44. Two-dimensional plot of the nickel and chromium dependence of swelling in Fe– Cr–Ni alloys irradiated with 5 MeV Ni+ ions at 675 ◦C to a dose of 140 dpa. Swelling was measured by the step-height technique (after [19])

8.3 Void Growth Equation

409

Fig. 8.45. The effect of impurity trapping on the free energy of void nucleation. Upper curves are for vacancy trapping and lower curves for interstitial trapping. The nucleation rates calculated from the curves are given as a function of binding energy in eV (after [42])

While the potential exists for precipitates to strongly influence void growth through their action as sinks or recombination sites, measurements of the effect of precipitation on void growth have failed to show that they play a significant role. 8.3.11 Effect of Reactor Operating History Much of our understanding of void behavior in metals comes from irradiation in reactors. The experimental data is used to validate models and to provide material parameters to benchmark the models. Given that most models assume that reactor parameters (temperature, dose rate, stress) are constant over time, it is often

410

8 Irradiation-Induced Voids and Bubbles

Fig. 8.46. The effect of impurity trapping on void growth rates. Upper curves are for vacancy trapping and lower curves are for interstitial trapping (after [42])

true that in both commercial and test reactors, these parameters can vary considerably during operation and due to the shutdown-startup cycle. It is not unusual for irradiation experiments to experience numerous power (and hence, temperatures) reductions over the course of a sixth month to one year irradiation. Garner [47] cites one instance in which a 600 ◦C, three-year irradiation experienced 237 temperature setbacks in the first year, during which the temperature fell to as low as 50 ◦C. While the dose accumulated at these lower than target temperatures is low (0.12 dpa in the 3.5 dpa accumulated in year 1), they can have a profound effect on the mi-

8.3 Void Growth Equation

411

Fig. 8.47. The fraction of traps occupied for vacancy trapping at typical charged particle and fast reactor dose rates and temperatures vs. binding energy. Under these conditions, the fraction of traps occupied is small even at high vacancy binding energies (after [42])

crostructure. Figure 8.51a shows the difference of dislocation loop size and number density in Ni–2.0Si samples irradiated in JMTR at 400 ◦C for the case of “conventional” temperature control vs. one where the temperature control was considerably improved. The smaller mean loop size and larger density is likely the result of additional loop nucleation during the periods where temperature was low but the neutron flux was non-zero. This low-temperature microstructure persisted at the nominal irradiation temperature and resulted in an alteration of the loop size distribution as compared to the case in which temperature was controlled. Low-temperature loop nucleation in a high temperature microstructure can also affect the evolution of the void microstructure. Figure 8.51b shows the microstructure of a Fe–15Cr–16Ni alloy irradiated at 600 ◦C in the Materials Open Test Assembly (MOTA) in the Fast Flux Test Facility (FFTF) to comparable doses. The sample on the left was in an assembly, reactor shutdown occurred over a six-hour period during which the temperature was reduced by 50 – 100 ◦C and then to gradually over the six-hour period during which the flux was also decreased. Irradiation during cooling is responsible for the formation of the fine dislocation loop structure. Following rapid shutdown during which the neutron flux and temperature is decreased over a several minute period, no fine loop structure is observed. The fast drop in temperature does not provide an opportunity to accumulate enough dose in this intermediate temperature regime to cause loop nucleation.

412

8 Irradiation-Induced Voids and Bubbles

Fig. 8.48. Influence of (a) silicon and (b) phosphorus on the swelling in EBR-II of annealed Fe–25Ni–15Cr at various combinations of temperature and fluence (after [43])

8.3 Void Growth Equation

413

Fig. 8.49. Influence of phosphorus level on swelling in EBR-II for a titanium-modified 316 steel at 425 and 540 ◦C (after [44])

Fig. 8.50. Suppression of swelling to at least 50 dpa in 316 SS doped with ∼ 1 wt% Hf after irradiation with 5 MeV Ni++ ions at 500 ◦C (after [45])

414

8 Irradiation-Induced Voids and Bubbles

Fig. 8.51. (a) Effect of temperature control on dislocation loop formation and growth in Ni–2%Si irradiated at 400 ◦C in the Japan Materials Test Reactor (JMTR) to a dose of ∼ 1024 n/m2 . LHS is convential control (0.92 ×1024 n/m2 , E > 1, 0 MeV), RHS is improved control (0.96 ×1024 n/m2 ). (b) Effect of shutdown rate on the formation of small dislocation loops in Fe–15Cr–16Ni irradiated at in FFTF at 600 ◦C. The image on the left underwent a slow temperature decrease during power shutdowns compared to a very rapid reduction in temperature at shutdown for the sample on the right (after [47])

The significance of these observations is twofold. First, that a low-temperature dislocation microstructure introduced into a high-temperature microstructure can alter the further development of that microstructure, affecting both loop and void evolution. Second, only very small doses (< 0.1 dpa) are required to nucleate the fine loop structure that remains stable during the continuation of the irradiation at high temperature. This data also provides additional information on the loop nucleation rate, indicating that it is perhaps higher than current models can explain.

8.4 Bubble Growth

415

8.4 Bubble Growth Up to this point, we have been treating voids as essentially empty cavities that grow and shrink by the absorption of vacancies. We have accounted for the effect of gas atoms on the nucleation of voids and also on the equilibrium vacancy concentration at the void surface. But we have not discussed the magnitude of the pressure in the void due to the gas and the effect this may have on the growth of the void. We also have made no distinction between a void and a bubble. One question that we would like to answer is how much gas must a void have in order to be considered a bubble? In a practical sense, the distinction is largely one of degree and character. A cavity is considered to be a bubble if the effect of the gas (on the surface energy and due to the pressure) causes the cavity to become spherical. This is essentially how voids and bubbles are distinguished in transmission electron microscopy. Due to the periodicity of the lattice, cavities will be faceted with the facets lying on the close-packed planes. But if the surface energy is changed by the gas, or if the gas pressure is high enough, then the cavity will become spherical in shape. Of course, very large voids will approach a spherical shape as the contribution of the facets diminishes with increasing void radius. Because insoluble gases are often formed by transmutation when certain elements are irradiated, inert gas bubbles form, which alter the mechanical and physical properties of an alloy. Bubble formation depends on the mobility of the gas (either in the form of individual atoms or complexes), the minimum number of gas atoms which are able to form a stable nucleus and the rate at which lattice vacancies can be supplied to enhance the stability of a nucleated core. Bubbles nucleate under irradiation and then grow or redissolve. The criterion is that nucleation ceases when a gas atom diffusing at random is most likely to encounter a pre-existing nucleus rather than take part in creating a new one. The resulting bubble density varies inversely as the square root of the gas atom diffusion coefficient and thus increases with decreasing temperature. The following assumptions about bubble nucleation under irradiation are made. Homogeneous nucleation is predicated on the premise that bubbles grow by the interaction of gas atoms from a background atomic population on a random basis. Thus, no account is taken of local effects such as cascade processes or precipitation on lattice defects or impurity agglomerates. Concerning stable nuclei, we assume that a pair of gas atoms is stable against thermal dissociation and that its activation energy is such that its motion may be ignored with respect to that of single gas atoms. In this section, we will first consider the mechanics of bubbles followed by the development of bubble growth models that will closely parallel void growth. 8.4.1 Bubble Mechanics For a gas-filled bubble of radius R, embedded in a solid medium, the change in the free energy of the solid due to the bubble is: dG = V dp + γ dA .

(8.188)

416

8 Irradiation-Induced Voids and Bubbles

Since V dp = d(pV ) − p dV ,

(8.189)

and for an ideal gas, pV = constant and V = 4/3π R3, then: dG 2γ = −4π R2 p − . dr R

(8.190)

Setting dG/ dr = 0 yields: p = 2γ /R .

(8.191)

Thus, the equilibrium condition for a bubble is expressed by the force balance p = 2γ /R, in which the force due to the outward pressure of the gas, p, is balanced by the inward-acting force due to the surface tension, 2γ /R. In the presence of a stress, the force balance becomes: 2γ −σ . (8.192) p= R where positive stress is tension. All bubble models require a specific relation between the number of gas atoms in a bubble and its radius. The van der Waals equation of state is used to describe the thermodynamic state of inert gas in bubbles. Letting nx be the number of gas atoms in a spherical bubble of radius R and the gas density is ρg . Then: nx = (4/3π R3)ρg .

(8.193)

From the idea gas law (pV = nkT ), we have: p

V = kT n

or

p = kT ρg

or

p=

3nkT . 4 π R3

(8.194)

Using Eq. (8.191) for mechanical equilibrium to eliminate ρg and p in Eqs. (8.193) and (8.194) gives: nx = 4/3π R3

2γ RkT

(8.195) 8 π R2 γ . 3kT For small R, 1/ρg is not proportional to R and we must account for the volume occupied by the gas atoms themselves. We do this by modifying Eq. (8.194) to include a term B which is a function of temperature and pressure. This gives us van der Waals equation of state: kT 1 1 − B = kT or = B+ P R, (8.196) ρg ρg 2γ =

and Eq. (8.195) becomes: nx =

4/3π R3 8 π R2 γ = . 3(kT + 2Bγ /R) B + (kT /2γ )R

(8.197)

8.4 Bubble Growth

417

For large R, the perfect gas approximation applies, and for very small R, the dense gas limit applies. Physically, there is a minimum volume occupied by each atom, B and as R decreases, the volume per atom approaches this limit. The result is: nm3 1 : dense gas limit , =B ρg atom and 1 ∼ = ρg

kT 2γ

(8.198)

R : ideal gas limit .

(8.199)

Note that for stainless steel at 500 ◦C, where γ ∼ 1.75 J/m2, 2γ /kT ∼ 328 nm−2 and 1 ∼ nm3 . = 3 × 10−4R ρg atom The limiting cases corresponding to Eqs. (8.198) and (8.199) are: 4 π R3 nx = for small R (8.200) 3B 2γ 4 π R2 for large R . (8.201) = 3 kT If Eq. (8.191) is not satisfied, then the bubble is described as a non-equilibrium bubble. That is, the bubble is not in equilibrium with the solid. Mechanical equilibrium is usually maintained by a flow of vacancies to the bubble to provide the additional volume needed to accommodate the influx of gas atoms. Whether Eq. (8.191) is satisfied depends on the relative absorption rates of vacancies and gas atoms by the bubble. A bubble of radius R can be considered as the absence of (4/3π R3)/Ω matrix atoms where Ω is the atomic volume. The empty sphere of radius R can be thought of as consisting of nv vacancies given by: nv =

4/3π R3 . Ω

(8.202)

The number of gas atoms in a sphere of radius R in mechanical equilibrium is given by Eq. (8.197). The number of vacancies per gas atom in an equilibrium bubble is then: kT R nv B = + . (8.203) nx 2γ Ω Ω Note that nx increases as R2 but nv increases as R3 , so increasing numbers of vacancies are needed per gas atom in order to maintain equilibrium. Stress is accounted for by taking Eq. (8.192) and substituting in from Eq. (8.194) for p gives:

σ=

2γ 3nx kT − , R 4 π R3

(8.204)

418

8 Irradiation-Induced Voids and Bubbles

where σ is the hydrostatic tensile stress. The critical bubble radius for unstable bubble growth is determined by setting dσ / dr = 0 and solving for R, yielding: Rc =

9nx kT 8πγ

1/2 .

(8.205)

Substituting for Rc in Eq. (8.205) into Eq. (8.204) gives:

σc =

128πγ 3 81nx kT

1/2 ,

or nx =

128πγ 3 . 81σc2 kT

(8.206)

The critical bubble radius, Rc is related to the equilibrium bubble radius, R0 by expressing Eqs. (8.201) and (8.205) in terms of the number of gas atoms in the bubble, nx and eliminating nx , giving: √ Rc = 3R0 , (8.207) and the critical stress in terms of R0 is: √ 4 3γ σc = . 9R0

(8.208)

Substituting for Eq. (8.201) into Eq. (8.204) to eliminate nx gives a relation between the applied stress, the initial bubble size and the critical bubble size: R20 2γ σc = 1− 2 . (8.209) Rc Rc Equations (8.208) and (8.209) provide the bubble stability criterion in terms of the applied stress and the bubble size. For bubbles of size R0 , Eq. (8.208) gives the critical stress for stability. For a solid with bubbles of size R0 < Rc , application of a tensile stress σc will cause the bubble to grow to size Rc specified by Eq. (8.209). If R0 > R or if σc is greater than the right hand side of Eq. (8.208), then the bubble will grow without bound. Or, for a given applied stress, Eq. (8.208) gives the critical bubble radius for stability. Equation (8.205) can be compared to the stability equation for a gas-free void in a solid subject to a stress, σ . For p = 0 in Eq. (8.192), we have that σ = 2γ /R. The numerical coefficient in Eq. (8.208) is about 0.77, which is less by about a factor of 3 than the coefficient for the void. The difference is due to the effect of the gas pressure in the bubble that assists the stress. 8.4.2 Growth Law Analogous to void growth, the time rate of change of the volume of a bubble is equal to the difference in the rates at which vacancies and interstitials are absorbed and to the volume carried by each of these point defects: d 4 3 π R = Ω 4π RDv Cv − CvV − 4π RDi Ci − CiV , (8.210) dt 3

8.4 Bubble Growth

419

and so the growth law is: dR Ω ≡ R˙ = Dv Cv − CvV − Di Ci − CiV , dt R

(8.211)

where CvV and CiV are the concentrations of vacancies and interstitials at the bubble surface and Cv and Ci are the point defect concentrations in the bulk solid. The thermodynamic vacancy concentration at the bubble surface given by Eq. (8.85) is modified to include the effect of gas pressure in the bubble:

−Ω 2γ CvV = Cv0 exp p− , (8.212) kT R and for interstitials

Ω 2γ V 0 Ci = Ci exp p− , kT R

(8.213)

where Cv0 and Ci0 are the thermodynamic equilibrium concentrations of vacancies and interstitials respectively for a stress-free solid and the exponential terms reflect the presence of a mechanical stress acting on the solid equal in magnitude to p − 2γ /R. Because Ci0 is so small, the interstitial term, Eq. (8.213) can be neglected. Setting dR/ dt = 0 in Eq. (8.211) and substituting Eq. (8.212) for CvV into the resulting expression, taking logarithms and re-arranging gives [48, 49]: Rc =

2γ , kT p+ ln Sv Ω

(8.214)

where Sv is the effective vacancy supersaturation given by: Sv =

DvCv − DiCi . DvCv0

(8.215)

Now, substituting Eq. (8.194) for p into Eq. (8.214) and re-arranging gives: g(Rc ) = R3c −

2γΩ 2 3nx Ω Rc + =0, kT ln Sv 4π ln Sv

(8.216)

where the expression is denoted by the function g(Rc ), which is zero when Rc is a root. The growth rate is plotted as a function of void radius in Fig. 8.52 for three conditions. The lower curve is the case where Eq. (8.216) has three real roots, the middle curve shows the case in which at least two of the roots are equal and the upper curve has one real root [49]. In case I, the roots are denoted RBc and RV c . A void B containing enough gas atoms that it is between RBc and RV c will shrink back to Rc . B A void with the same number of gas atoms but with radius below Rc will grow to RBc and stop. Finally, a void with the same number of gas atoms and with radius above RV c will grow without limit by bias-driven growth. As the number of gas atoms increases, Eq. (8.216) is represented by curves that progress from I to II to III. In

420

8 Irradiation-Induced Voids and Bubbles Fig. 8.52. Schematic plot of cavity growth rate as a function of cavity radius for increasing amount of helium gas in the void or Sv (after [48])

the case of curve III, the number of gas atoms is large enough that there will be no intersections with the dR/ dt = 0 axis and these cavities will only grow by biasdriven growth. At some critical number of gas atoms, there is just one intersection of the function dR/ dt with the dR/ dt = 0 axis. This case is represented by curve II. In this case, the corresponding number of gas atoms is denoted as n∗x and the ∗ corresponding minimum critical radius where RBc and RV c coincide is denoted as Rc . ∗ The quantity, nx is the maximum number of gas atoms that may be contained in a cavity for there to still exist a critical radius, with a minimum value of R∗c . The minimum critical radius, R∗c can be found by taking the derivative of Eq. (8.216) with respect to Rc , giving: 4γΩ dg(Rc ) = 3R2c − Rc . dRc kT ln Sv

(8.217)

Setting Eqs. (8.216) and (8.217) to zero simultaneously yields the minimum critical radius: R∗c =

4γΩ , 3kT ln Sv

(8.218)

and from Eq. (8.205): n∗x =

128πγ 3Ω 2 . 81(kT )3 (ln Sv )2

(8.219)

Stoller et al. [49] noted that Eq. (8.219) can be written for non-spherical cavities using a shape factor, FV such that: n∗x =

32FV γ 3 Ω 2 , 27(kT )3 (ln Sv )2

(8.220)

8.4 Bubble Growth

421

where FV = 4π /3 for a spherical void. He also notes that more physically reasonable solutions are obtained using a hard-sphere equation of state rather than the ideal gas law, which tends to overpredict swelling incubation times. It should also be noted that Eqs. (8.219) and (8.206) are the same when σ is replaced with Ω / ln S, indicating that the stability criterion is the same regardless of whether the solid is acted on by an actual stress or an effective stress defined by the irradiation-induced vacancy supersaturation. A bubble is stable for negative vacancy supersaturation and can be stable or metastable for positive vacancy supersaturation depending on the magnitude of the supersaturation, the gas content and the bubble size according to Fig. 8.52. For a constant stress or irradiation-induced vacancy supersaturation, when the stability limit is reached by gas absorption, a bubble starts to grow by vacancy absorption and is transformed into a cavity. Equations (8.218) and (8.205) describe the bubble-to-void conversion criterion. Equation (8.211) can be used to calculate the swelling rate due to bubble swelling by assuming all gas to be in the bubbles, re-solution to be insignificant and the gas to be ideal such that: p=

nx kT , 4/3π R3ρB

(8.221)

where ρB is the total bubble density and nx = xt ˙ is the gas concentration in the solid being produced by transmutation at a rate of x. ˙ The swelling rate due to bubble growth is: d(ΔV /V )/ dt = (4π R2ρB /Ω ) dR/ dt .

(8.222)

8.4.3 Bubble Growth by Dislocation Loop Punching While vacancy diffusion is the prime mechanism contributing to bubble growth on a fine scale, an additional mechanism for bubble growth in the case of high gas pressure is dislocation loop punching. If the pressure in the bubble is large enough, the stress in the solid nearby may reach a level where dislocation sources can be activated, resulting in the growth of the bubble by punching out a dislocation loop (Fig. 8.53). Recall that the stress required to operate a Frank–Read source is ∼ μ b/l, where l is the spacing between pinning points. Dislocation sources that are easiest to activate will be those with l ∼ r0 , where r0 is the radius of the bubble. So the excess pressure required for the bubble to generate dislocations is then ∼ μ b/r0 . The magnitude of the excess pressure required to generate prismatic dislocations can be determined by comparing the free energy change of the bubble upon creation of a dislocation loop of size equal to the bubble, to the energy of the loop itself [51]. The work to increase the bubble size is: 2γ π r02 b , (8.223) ΔF = −p dV = − p − r0 where p is the pressure in the bubble, V is the bubble volume, γ is the surface energy and b is the Burgers vector. Neglecting the stacking fault energy contribution, the

422

8 Irradiation-Induced Voids and Bubbles

Fig. 8.53. Schematic illustration of the growth of a bubble by dislocation loop punching (after [50])

energy of the prismatic dislocation loop of radius r0 given by Eq. (7.64) is approximated as: EL =

4r0 μ b2 r0 ln , 2(1 − ν ) rc

(8.224)

so that for dislocation loop formation to be energetically possible: p−

2γ r

π r02 b >

4r0 μ b2 r0 ln , 2(1 − ν ) rc

(8.225)

or approximating EL as π μ b2 r0 : p > (2γ + μ b)/r0 .

(8.226)

For typical values of γ and μ , the gas pressure in the bubble must be about an order of magnitude greater that 2γ /r0 before dislocations can be generated and allow the bubble to expand. 8.4.4 Bubble Lattices Similar to void lattices described earlier, high levels of He can result in the organization of gas bubble lattices. In fact, gas bubble lattice formation has been observed in bcc, fcc and hcp metals following He injection at temperatures < 0.3Tm [52]. Helium bubbles in Cu are aligned with dense-packed rows parallel to matrix {111} directions. Johnson et al. [52] measured the lattice constant of the He bubble superlattice in Cu to be aHe = 7.6 nm, corresponding to a bubble density of 1025 bubbles/m3 . Figure 8.54 shows a bright field transmission electron micrograph of a helium gas bubble lattice in molybdenum following 40 keV He+ irradiation to a dose of 5 ×1021 He+ /m2 at 500 ◦C. While the same forces driving the formation of void lattices is expected to apply to bubble lattices, additional interactions may arise due to the close spacing of overpressurized bubbles, such as bubble growth by dislocation loop punching.

Nomenclature

423

Fig. 8.54. He gas bubble superlattice formed in molybdenum following 40 keV He+ irradiation to a dose of 5 ×1021 He+ /m2 at 500 ◦C (after [39])

8.4.5 Helium Production An important ingredient in bubble formation and growth is the production of helium. In a reactor, He production is governed by the boron and nickel contents of the alloy through the reactions: 10

B(n, α )7 Li ,

(8.227)

and the two-step reaction: 58

Ni(n, γ )59 Ni(n, α )56 Fe .

(8.228)

The thermal neutron (n, α ) cross section for 10 B is very large, about 3837b, while the cross section for 59 Ni is for fast neutrons and is only about 4.3b. For thermal reactors then, a large amount of helium is produced early in life from transmutation of boron, but this source burns out by about 1 dpa (∼ 1021 n/cm2). The presence of nickel in stainless steels provides a smaller but sustained source of helium at higher dose. In this regard, thermal reactors produce greater amounts of helium at low dose and in a lower dose rate environment, making low dose helium-induced swelling a greater problem in a thermal reactor than in a fast reactor. Figure 8.55 shows the production rate of helium from an alloy containing 58 Ni and 10 B in the HFIR (thermal) reactor. Note that the production rate of helium is dominated at low fluence by the contribution from 10 B, and at higher fluence by 58 Ni. Helium buildup for the same alloy in a fast reactor and a fusion reactor are shown for comparison. Note that the helium buildup in a fusion reactor matches that in HFIR, and both are higher than that in a fast reactor.

424

8 Irradiation-Induced Voids and Bubbles Fig. 8.55. Helium buildup vs. fluence for stainless steel in HFIR (thermal reactor), a fusion reactor spectrum and a fast reactor spectrum. In the figure, r is the atom fraction of boron or nickel in the alloy and q is the initial fraction of the isotope listed in the figure (after [27])

Nomenclature a AXv,i B Cj C0j CvL dabs d c,e Dj Dc De Ds E Ebj Efj Emj FV g(Rc ) G G0 ΔG ΔG0n ΔGn H J k

Lattice constant Absorption rate of vacancies, interstitials by sink X Volume occupied by a gas atom in a lattice Concentration of species j Thermal equilibrium concentration of species j Vacancy concentration in equilibrium with a dislocation loop Effective diameter of dislocations for absorbing glissile SIA clusters Strength of diffusive spread for clusters (c) or for vacancy emission (e) relative to single point defects Diffusion coefficient of species j Diffusive spread due to cascades Diffusive spread due to vacancy emission Diffusive spread due to single defect jumps Energy Binding energy of specie j Formation energy of specie j Migration energy of specie j Shape factor (= 4π /3 for spherical void) Void growth rate factor, defined in Eq. (8.216) Free energy Free energy of perfect lattice Change in free energy Activation barrier for void nucleation without interstitials Activation barrier for void nucleation with interstitials Enthalpy, also Henry’s law constant Eq. (8.57) Nucleation current Boltzmann’s constant

Nomenclature

kg2 kX2 k2j Kcleff Kj Kiv K eff j K0 K0eff Kxc l Lj mi M Mx n ncr nk , nk nv,i Nd j N0 NR NS p pcl pl Pm Q r r0 R Rg Rc Rcr Riv Rmax R0 R˙ rk , rk S Sj T V

Sink strength for 1D diffusing SIA clusters Sink strength of sink X Total sink strength species j Effective production rate of defects in clusters and free form Loss rate of species j Vacancy–interstitial recombination rate Effective production rate of free defects of type j Defect production rate Effective Frenkel Pair production rate accounting for recombination Rate of gas atom re-solution Distance of cluster to a grain boundary Thermal emission rate of species j Number of interstitial in an interstitial loop Helium concentration Helium cluster of x gas atoms Number of vacancies in a void Number of vacancies in a void of critical size Critical void nucleus cluster size Number of vacancies, interstitials Average number of defects of type j generated in a single cascade Number of lattice sites per unit volume See Eq. (8.151) See Eq. (8.154) Gas pressure Defined in Eq. (8.186) Defined in Eq. (8.185) Probability of nucleating a void embryo of size m Defined in Eq. (8.148) Radius Prismatic dislocation loop radius Void or bubble radius Grain radius Critical bubble radius Critical void radius Vacancy–interstitial recombination rate Saturation void size Equilibrium bubble radius Rate of change of radius, growth rate Critical void nucleus radius Entropy Supersaturation of species j Temperature Volume

425

426

8 Irradiation-Induced Voids and Bubbles

ΔV /V wn x xg zv zi Z Z

Fractional volume Number of ways of removing ρ 0 (n) voids of size n from a solid Number of gas atoms in a void Mean glissile cluster size Vacancy bias factor Interstitial bias factor Zeldovich factor Zeldovich factor in the presence of interstitials or in a stressed solid

αj β βj δ εig εT Φ γ η μ μx ν θ Θ ρ ρx σ τ Ω ξ ζ

Emission rate of species j 2γΩ /kT defined in Eq. (8.71) Absorption rate of species j Thickness of void shell Fraction of interstitials in glissile clusters Fraction of Frenkel pairs that recombines during cascade cooling Fluence or dose Surface energy Defined in Eq. (8.117) Shear modulus Chemical potential of species x Poisson’s ratio Angle between surface and tangent to void, Eq. (8.81) Defined in Eq. (8.98) Void size distribution Density of entity x Hydrostatic stress Time Atomic volume Defined in Eq. (8.15) Defined in Eq. (8.130)

Subscripts B cr CP D g gb hom i j IP L N

Bubbles Critical size Coherent precipitates Total dislocations Glissile clusters or gas Grain boundary Homogeneous Interstitials Defect specie representation Incoherent precipitates Dislocation loops Network dislocations

Problems

s v V 0

427

Sinks Vacancies Void Equilibrium

Superscripts c e L m s V 0

Cascades Vacancy emission Loops Number of vacancies in a void embryo of size m Single defects Voids Equilibrium Minimum critical value In presence of interstitials

∗

Problems 8.1 In a solid where the effect of interstitials are neglected (i.e., where βi /βv = 0), a) Determine the critical void embryo size (in terms of the number of vacancies and void radius). b) Show schematically how the number of vacancies in the critical size void embryo varies with: i) Temperature ii) Degree of vacancy supersaturation iii) Void surface energy iv) The presence of interstitials c) How do your answers to parts (a) and (b) change when an inert gas is present? 8.2 Determine the critical void embryo size for 316 stainless steel (a = 0.3 nm, γ = 1.75 J/m2) irradiated at 500 ◦C so as to produce a vacancy supersaturation of 103 . 8.3 Derive Eq. (8.40). ˙ o for stainless steel (Tm = 8.4 Calculate and plot the relative void growth rate R/R 1823 K) as a function of T /Tm , given that Qvf = 1.4 eV Qvm = 1.09 eV

ρd = 1010 cm−2 Σs = 0.3 cm−1 φ = 1014 n/cm2 s ν = 100 displacements/neutron

428

8 Irradiation-Induced Voids and Bubbles

ziv = 30 Zi = 1.02 Zv = 1.00 a3 = Ω = 0.011 nm3 kT /2γ = 0.01 nm2

ν = 1013 s−1 Neglect voids as sinks (ρV 0) and precipitates (ρCP ∼ 0) and loops as sinks (ρL 0). Assume the vacancy diffusion coefficient is given by Dv = ν a20 exp(−Qvm /kT ) and the equilibrium vacancy concentration is given by Cv = Ω −1 exp(−Qvf /kT ) . Assume the void diameter is 50 nm. 8.5 The equation for growth of a cavity is given by: dR Ω = Dv (Cv − CrV ) − DiCi . dt R Explain what happens to the cavity growth rate if the radiation dose rate doubles. Assume low sink strength and low temperature. Explain what happens if the radiation stops but the sample is held at the same temperature that existed during the radiation. 8.6 A solid is subjected to a neutron flux, resulting in void formation and growth. At time t1 , a condition is reached where the dislocation density is 109 cm−2 , the voids are all 100 nm in diameter at a density of 1014 cm−3 and the void growth rate is zero. In the absence of thermal emission, however, R˙ = 10−2 nm/s. The metal is instantaneously strained such that the dislocation density increases by a factor of 10 and the void growth rate in the absence of thermal emission increases to 8 ×10−2 nm/s. Determine the direction and magnitude of the hydrostatic stress needed to suppress void growth. Assume that the solid contains no dislocation loops or precipitates and that the voids are gas-free. 8.7 Pure nickel has been found to be highly susceptible to void formation when irradiated in a fast neutron spectrum. Along with voids, perfect dislocation loops are found in nickel. In comparison, Fe–18Cr–8Ni stainless steel is less susceptible to void formation and faulted Frank loops are found; but voids are also present. As the nickel content in the stainless steel is increased, two other observations are made. The susceptibility to void formation decreases, and voids that are present are surrounded by a nickel-rich shell.

Problems

429

Given the following information, explain each of these observations.

σ /γ |Ni < σ /γ |Fe , Element σeff (n, α )

RNi < RFe

Cr 0.20

Fe 0.23

Ni 4.20

8.8 a) Explain the reason for the characteristic bell-shaped plot of swelling vs. irradiation temperature. b) How and why is the shape changed by: i) Cold-work prior to irradiation ii) The addition of impurities iii) Grain size c) Explain why swelling and creep can affect each other. 8.9 You are designing the stainless steel fuel cladding for the Advanced Breeder Reactor. Your objective is to delay void nucleation and minimize void growth. Concerning cladding fabrication, you can control: a) Grain size b) Degree of cold-work c) Precipitate density d) Impurity content of the steel. From a design standpoint, you can control the normal operating temperature of the cladding over a window of 100 ◦C. Using void nucleation and growth theory, how can you utilize these five parameters to reach this goal? Be quantitative where possible. 8.10 Annealing is a means of removing radiation damage from an alloy. For stainless steel with both dislocation loop and void populations, explain what will occur when the steel is annealed at 600 ◦C for several hours. In describing the changes during annealing, indicate relative rates and endpoints. 8.11 In the absence of gas atoms, we wish to eliminate voids in Cu by thermal treatment at 400 ◦C. Calculate the length of time needed to accomplish this for an initial void radius of 5 nm and 30 nm. The surface free energy of copper is 1.73 J/m2. 8.12 Given that the number of gas atoms in a bubble can be described as m = (4/3π R3)ρg and that the gas atom density, ρg , can be described by 1/ρg = B + (kT /2γ )R where B is the dense gas limit: a) Show that the volume increase that accompanies coalescence of equal size gas bubbles is given as (ΔV /V )final /(ΔV /V )initial = /2 .

430

8 Irradiation-Induced Voids and Bubbles

b) Assuming that the overall gas balance in UO2 can be given as Y F t = mN where Y = noble gas yield of a fission event F = fission rate density m = gas atoms per bubble N = bubble density, and all the gas remains in bubbles. Develop an expression for the volumetric swelling rate and indicate the dependence on burnup. c) How would you account for i) Gas remaining in the matrix? ii) Re-solution?

References 1. Cauthorne C, Fulton E (1967) Nature 216:575 2. Jenkins ML, Kirk MA (2001) Characterization of Radiation Damage by Transmission Electron Microscopy. Institute of Physics Publishing, Philadelphia, PA 3. Adda U (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 31 4. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Center, USERDA, Washington, DC 5. Mansur LK (1994) J Nucl Mater 216:97–123 6. Russell KC (1971) Acta Met 19:753 7. Powell RW, Russell KC (1972) Rad Eff 12:127 8. Katz JL, Wiedersich H (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 825 9. Russell KC (1979) Acta Met 26:1615 10. Packan NH, Farrell K, Stregler JO (1978) J Nucl Mater 78:143 11. Wiedersich H, Katy JL (1979) Adv Colloid Interface Sci 10:33 12. Russell KC (1972) Acta Met 20:899 13. Katz JL, Wiedersich H (1973) J Nucl Mater 46:41 14. Semenov AA, Woo CH (2002) Phys Rev B 66:024118 15. Brailsford AD, Bullough R (1972) J Nucl Mater 44:121–135 16. Mansur LK (1978) Nucl Technol 40:5–34 17. Brimhall JL, Kissinger HE, Kulcinski GL (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 338 18. Garner FA, Porollo SI, Vorobjev AN, Konobeev YuV, Dvoriashin AM (1999) In: Ford FP, Bruemmer SM, Was GS (eds) Proceedings of the 9th International Symposium on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, The Minerals, Metals and Materials Society, Warrendale, PA p. 1051 19. Garner FA (1984) Irradiation performance of cladding and structural steels in liquid metal reactors, chap 6. In: Frost BRT (ed) Materials Science and Technology, vol 10A, Nuclear Materials, part I. VCH, New York

References

431

20. Krasnoselov VA, Prokhorov VI, Koleskikov AN, Ostrovskii ZA (1983) Atomnaya Energiya 54(2)111–114 21. Garner FA, Bates JF, Mitchell MA (1992) J Nucl Mater 189:201–209 22. Brager HR, Garner FA (1979) Effects of Radiation on Structural Materials the 9th International Symposium, STP 683. America Society for Testing and Materials, Philadelphia, PA, 1979, pp 207–232 23. Dupouy JM, Lehmann J, Boutard JL (1978) In: Proceedings of the Conference on Reactor Materials Science, vol. 5, Alushta, USSR. Moscow, USSR Government, pp 280–296 24. Busboom HJ, McClelland GC, Bell WL, Appleby WK (1975) Swelling of Types 304 and 316 Stainless Steel Irradiated to 8 × 1022 n/cm2 , General Electric Company Report GEAP-14062. General Electric Co., Sunnyvale, CA 25. Seran LJ, Dupouy JM (1982) In: Effects of Radiation on Materials the 11th International Symposium, STP 782. American Society for Testing and Materials, Philadelphia, PA, 1982, pp 5–16 26. Seran LJ, Dupouy JM (1983) In: Proceedings of the Conference on Dimensional Stability and Mechanical Behavior of Irradiated Metals and Alloys, vol 1, Brighton. British Nuclear Energy Society, London, 1983, pp 22–28 27. Mansur LK (1993) J Nucl Mater 206:306–323 28. Brailsford AD, Bullough R (1973) J Nucl Mater 48:87 29. Brailsford AD, Bullough R (1972) British Rep AERE-TB-542 30. Dubuisson P, Maillard A, Delalande C, Gilbon D, Seran JL (1992) Effects of Radiation on Materials the 15th International Symposium, STP 1125. American Society for Testing and Materials, Philadelphia, PA, 1992, pp 995–1014 31. Brager HR, Garner FA, Guthrie GL (1977) J Nucl Mater 66:301–321 32. Wolfer WG, Foster JP, Garner FA (1972) Nucl Technol 16:55 33. Brailsford AD (1975) J Nucl Mater 56:7 34. Wolfer WG, Mansur LK (1980) J Nucl Mater 91:265 35. Allen TR, Cole JI, Gan J, Was GS, Dropek R, Kenik EA (2005) J Nucl Mater 341:90–100 36. Singh BN, Golubov SI, Trinkaus H, Serra A, Osetsky Y, Baraskev AV (1997) J Nucl Mater 251:107–122 37. Golubov SI, Singh BN, Trinkaus H (2000) J Nucl Mater 276:78–89 38. Abromeit C (1994) J Nucl Mater 216:78–96 39. Ghoniem NM, Walgraef DJ, Zinkle S (2002) Comput Aided Mater Des 8:1–38 40. Woo CH, Frank W (1985) J Nucl Mater 137:7 41. Garner FA (1984) J Nucl Mater 122–123:459–471 42. Mansur LK, Yoo MH (1978) J Nucl Mater 74:228–241 43. Garner FA, Kumar AS (1987) Radiation-Induced Changes in Microstructure the 13th International Symposium, STP 955 (Part 1). American Society for Testing and Materials, Philadelphia, PA, 1987, pp 289–314 44. Garner FA, Brager HR (1985) J Nucl Mater 133–134:511–514 45. Gan J, Simonen EP, Bruemmer SM, Fournier L, Sencer BH, Was GS (2004) J Nucl Mater 325:94–106 46. Brailsford AD, Mansur LK (1981) J Nucl Mater 103–104:1403–1408 47. Garner FA, Sekimura N, Grossbeck ML, Ermi AM, Newkirk JW, Watanabe H, Kiritani M (1993) J Nucl Mater 205:206–218 48. Mansur LK, Coghlan WA (1983) J Nucl Mater 119:1–25 49. Stoller RE, Odette GR (1985) J Nucl Mater 131:118–125 50. Evans JH (1978) J Nucl Mater 76–77:228–234 51. Trinkaus H (1983) Rad Eff 78:189–211 52. Johnson PB, Mazey DJ, Evans JH (1983) Rad Eff 78:147–156

9 Phase Stability Under Irradiation

Irradiation can have profound effects on the formation or dissolution of phases by alteration of the stability of those phases. The most direct way in which irradiation can alter phase stability is by causing local enrichment or depletion of solute such that the solubility limit is crossed. But irradiation can also dissolve phases by recoil dissolution, cause disordering by creating anti-site defects, and lead to nucleation and growth of distinct phases. Under specific conditions, irradiation can also lead to the formation of metastable phases including amorphization. Because the phase structure of an alloy can significantly affect the physical and mechanical properties of the material, understanding how irradiation affects phase stability is of great importance for engineering materials.

9.1 Radiation-Induced Segregation and Radiation-Induced Precipitation Radiation-enhanced diffusion (RED), discussed in Chap. 4, and radiation-induced segregation (RIS), presented in Chap. 6, explain how irradiation can increase the atomic transport of atoms in the alloy, and how the coupling between the vacancy and interstitial fluxes and the solute and solvent atoms can lead to enrichment or depletion of solute atoms at defect sinks such as the free surface, grain boundaries, dislocations, precipitate interfaces, etc. Enrichment or depletion of solute can lead directly to precipitate formation if the local solute concentration exceeds the solubility limit, or precipitate dissolution if the solute content is driven below the solubility limit. Recall that the temperature dependence of RIS is such that at low temperatures, RIS is minimal due to low defect mobility and the high recombination rate of vacancies and interstitials, limiting the number available to annihilate at sinks. At high temperature, the high equilibrium vacancy concentration leads to enhanced recombination and faster back diffusion, limiting the degree of RIS. However, at intermediate temperatures, significant participation of the solute in the defect fluxes results in pronounced segregation at sinks. Figure 9.1 shows how RIS can lead to precipitate formation or dissolution at a sink. Enrichment of a solute at a sink can raise the local concentration (Fig. 9.1a) above the solubility limit (shown as a dashed line in Fig. 9.1b) locally. The excess solute can then precipitate as a second phase. If a second phase is already present, then depletion of the solute (Fig. 9.1c) can lead to dissolution of that phase locally (Fig. 9.1d).

434

9 Phase Stability Under Irradiation

Fig. 9.1. Schematic illustration showing (a) enrichment of solute at a sink and (b) its corresponding elevation above the solubility limit, and (c) depletion of a solute at a sink and (d) its corresponding suppression below the solubility limit

A classic example of radiation-induced precipitate formation and dissolution is described in Sect. 6.1.2 and Fig. 9.2 and Fig. 9.3 for the case of RIS in solid solution Ni–Si and Ni–Al alloys. The consequence of a large amount of solute enrichment at sinks is precipitation of a second phase. In the Ni–Si system, Si is undersized relative to Ni and enriches at sinks during irradiation (Fig. 9.2). RIS causes segregation to levels that are well above the solubility of Si in Ni, resulting in formation of a Ni3 Si, γ precipitate. Ni3 Si precipitates at the surface, grain boundaries and dislocation loops. Conversely, in the case of Ni–Al, Al is oversized with respect to Ni and depletes at sinks under irradiation as shown in Fig. 9.3. The result is the dissolution of existing precipitates at those locations. Since the Ni–Al alloy is an initially homogeneous alloy and the Al content is below the solubility limit for Al, no precipitates are present before irradiation. However, as shown in Fig. 9.3, the region behind the depleted zone is enriched in Al and this amount of enrichment exceeds the solubility level at locations that are displaced from the sink interface, resulting in precipitation of Ni3 Al in a subsurface layer a small distance away from the grain boundary and dislocation loops. Both of these examples are consequences of crossing the solubility line for an element in solution by solute enrichment or depletion due to RIS, and constitute a primary mechanism of phase instability under irradiation.

9.1 Radiation-Induced Segregation

and Radiation-Induced Precipitation

435

Fig. 9.2. Formation of γ -Ni3 Si on defect sinks in a solid solution of Ni–6at% Si alloy showing (a) a surface coating of Ni3 Si, (b) toroidal γ precipitates at dislocation loops and (c) a grain boundary coated with Ni3 Si (from [1])

Fig. 9.3. Formation of γ Ni3 Al away from defect sinks in a solid solution of Ni–12.8 at% Al showing (a) a subsurface layer of γ Ni3 Al, and (b) formation of Ni3 Al away from dislocation loops (from [1])

436

9 Phase Stability Under Irradiation

9.2 Recoil Dissolution Atom displacements created within collision cascades can cause the atoms in a precipitate to be ballistically driven into the surrounding matrix, thus contributing to the dissolution of the precipitate. Nelson, Hudson and Mazey [2] developed a model (NHM) for recoil dissolution of precipitates that will be summarized here. For a displacement rate in the solid of K0 dpa/s, the flux of atoms (atoms per unit area per second) from the precipitate surface can be written as ζ K0 . For a spherical precipitate of radius rp , the dissolution rate expressed as the rate of volume shrinkage is given by: dV = −4π rp2 ζ K0 Ω , (9.1) dt where Ω is the atomic volume. Dissolution by recoil re-solution of the solute is balanced by growth of the precipitate due to diffusion of the solute atoms to the precipitate. Even though the solute is being re-distributed between the precipitate and the matrix, the total concentration of solute, C is fixed, and can be expressed as: C = 4/3π rp3ρ Cp + Cs ,

(9.2)

where ρ is the precipitate density and Cp is the concentration of solute in the precipitates and Cs is the concentration of solute in solution. The growth rate of precipitates due to the solute flux is given by: 3DCs rp dV = , dt Cp

(9.3)

where D is the solute diffusion coefficient. The net growth rate of the precipitate is then the sum of terms due to recoil dissolution, Eq. (9.1) and precipitate growth due to diffusion of solute from solution, Eq. (9.3) and can be written as: 3DCs rp dV = −4π rp2 ζ K0 Ω + . dt Cp

(9.4)

Substituting for Cs from Eq. (9.2) gives: 3DCrp dV = −4π rp2 ζ K0 Ω + − 4π rp4Dρ , dt Cp

(9.5)

and writing Eq. (9.5) as a radial growth law gives: drp 3DC − rp2 Dρ . = −ζ K0 Ω + dt 4π rpCp

(9.6)

Equation (9.6) is plotted in Fig. 9.4 and shows that for small precipitate sizes, the growth rate is positive, but at larger sizes where the surface area becomes large, precipitates will dissolve. At the size dictated by zero growth rate, dissolution is balanced by re-precipitation. Note that the effect of irradiation is to result in a type

9.2 Recoil Dissolution

437

Fig. 9.4. Growth rates for precipitates undergoing irradiationinduced dissolution (from [2])

of inverse coarsening in which smaller particles are more stable than larger ones, which is opposite that which occurs by Ostwald ripening. The solute concentration profile can be determined with the use of a cell model in which all precipitates are of the same size and each is in a matrix cell of radius, L with 4/3π L3ρ = 1. In the Wilkes model [3] re-solution deposits the solute atoms homogeneously throughout the cell and constitutes a source term in the steady state solution of the diffusion equation. Figure 9.5 shows the solute source term in the ∂C = D∇2C + ζ K0 , matrix surrounding the precipitate. The diffusion equation is ∂t

Fig. 9.5. Source terms for irradiation-induced re-solution of solute from the precipitate, according to various models. The term rp is the precipitate radius, L is the precipitate spacing, R is the recoil radius in the Frost–Russell model [10, 11], and δ is the shell about rp in the Brailsford model [4]

438

9 Phase Stability Under Irradiation

∂ C = 0 at the cell boundary (r = L), ∂ r r=L and the solute concentration at the precipitate surface equals the equilibrium concentration, C(rp ) = Ce , the concentration is then:

3 ζ K0 rp2 2L (r − rp ) 2 2 C(r) = Ce + − r + rp . (9.7) 2Ω D(L3 − rp3 ) rrp

and subject to the boundary conditions:

The concentration profile of Eq. (9.7) is plotted in Fig. 9.6a and shows that the solute concentration rises from the precipitate boundary, rp and levels out as it approaches the cell boundary, L. The steady state cell boundary concentration, C(L) can be written as an excess concentration: 2DΩ χ= (C(L) − Ce ) ζ K0 (9.8) 2(rp /L) − 3(rp /L)2 + (rp /L)4 , =L 1 − (rp/L)2 and is shown in Fig. 9.6b as a function of precipitate-to-cell radius ratio (r0 /L). Note that for a fixed cell size the cell boundary concentration initially increases since the steady state solute supersaturation is increasing with precipitate surface area. When the precipitate is large, the precipitate surface is close to the cell wall and the back diffusion becomes significant, thus causing a reduction in the concentration. For most practical situations, the volume fraction of precipitate is small so that the precipitate size distribution is to the left of the peak in Fig. 9.6b. As a result, small precipitates will experience a net loss of solute until steady state is reached. An improvement in the treatment of the source term in the simple NHM model is obtained by assuming that particles are spaced infinitely far from each other (dissolution–re-precipitation at one particle is unaffected by others), and that resolution occurs at a uniform rate in a shell of thickness δ around the particle of radius, rp (Fig. 9.5) [4]. For an initial precipitate size of r0 , the resulting size was found to be: 3δ 2 rp (3rp + 2δ ) Θ 3 3 r0 − rp = − , (9.9) 8π Dρp[(rp + δ )3 − rp3 )] 4π rp2 where Θ is the re-solution induced rate of precipitate volume change. The effect of irradiation in this model is to reduce the precipitate size from its original dimension by up to a factor of 2 [3]. Note that for the case where δ → ∞, the result reduces to that given in Eq. (9.6). This result can be compared to the well-known thermal coarsening behavior of precipitates described by Wagner [5] and Lifshitz and Slyosov [6]: r¯p3 − r¯03 =

8DCe γ Vm2 t , 9RT

(9.10)

where r0 is the initial average precipitate radius, Ce is the solubility of the precipitate of infinite radius, Vm is the molar volume, γ is the particle-matrix interface

9.2 Recoil Dissolution

439

Fig. 9.6. (a) Steady state solute concentration in the matrix from Eq. (9.7), and (b) steady state boundary concentration from Eq. (9.8) (from [3])

energy and R is the gas constant. Accounting for irradiation-induced re-solution and irradiation-enhanced diffusion the maximum stable particle size [7, 8, 9] is shown to be: 3aD 1/2 , (9.11) rmax = l f K0

440

9 Phase Stability Under Irradiation

where a is the lattice spacing, l is the linear dimension of the cascade, f is the fraction of solute atoms dissolved and the product l f is the shrinkage by re-solution [2]. When particles are initially larger than the maximum stable size, the maximum size decreases according to: rmax (K0 t) − rmax(K0 t0 ) = −l f K0 (t − t0 ) ,

(9.12a)

and when the initial particle sizes are much smaller than that given by the equilibrium size distribution, then the particle size increases according to: 3 3 rmax (K0 t) − rmax (K0 t0 ) = 9aD(t − t0 ) .

(9.12b)

Note that Eq. (9.12b) is similar to Eq. (9.10) for thermal coarsening. A modification to the Wilkes’s cell model is to provide a source term for the re-deposited solute that is more realistic than having it deposited uniformly in the cell (Wilkes [3]) or uniformly in a shell (Brailsford [4]). Frost and Russell [10, 11] model the rate of solute re-deposition in the matrix using the rate at which recoils originate in the matrix, which depends on the distance from the precipitate center, r according to: Θ 2 rp − (r − R)2 , (9.13) 4rR where Θ is the re-solution rate per atom and R is the recoil distance (Fig. 9.5). Solving the diffusion equation with the spatially dependent source term, G(r): G(r) =

∂C = D∇2C + G , ∂t gives: Θ 3 r − rp3 − 4R r2 − rp2 48RD 1 1 2 − , −6 rp − R2 (r − rp ) − (3rp − R)(rp + R)3 r rp

(9.14)

C(r) = C0 +

and the maximum concentration is given by: Θ R2 R . Cmax = C0 + 1− 12D 4rp

(9.15)

(9.16)

The maximum solute concentration is proportional to the re-solution rate and weakly dependent on the precipitate size. The inverse coarsening rate of particles that are not of the same size can be determined by calculating the diffusion near each particle [10, 11]. The calculation assumes that the concentration at the edge of its cell is an average matrix concentration, and that there is no net flux to or away from a precipitate of some radius, rm giving: rp 1 drp L Θ R3 = 1− , (9.17) 2 2 dt rm rp (L − rp ) 48

9.2 Recoil Dissolution

441

for which solutions exist depending on the value of rm . Assuming that rp L and the initial precipitate size is r0 , then: rp3 (t) r03 rp2 (t) r02

= 1+

t , τA

for rp rm

and τA =

48r03 , Θ R3

(9.18)

= 1−

t , τB

for rp rm

and τB =

24rm r02 , Θ R3

(9.19)

rp − rm = (r0 − rm ) exp(−t/τC ) ,

for r ∼ = rm

and τC =

3 48rm . Θ R3

(9.20)

Note that the relation between the particle size and time is rp3 α t when the size is below rm and rp2 α t when the size is greater than rm . For all cases, when R, r0 and rm are of the order of 10 nm, t is between 10/Θ and 100/Θ . For the case of fast reactor conditions, Θ ∼ 10−7 dpa/s, so 108 s ≤ t ≤ 109 s, which is equivalent to 3 to 30 years. Since the incubation time varies with r3 , larger precipitates would require even longer for inverse coarsening to occur. Consequently, irradiation-induced inverse coarsening by recoil re-solution is expected only after very long-term exposures. The effect of irradiation on precipitate stability is shown schematically in Fig. 9.7 as a series of illustrations with increasing dose. Prior to irradiation, the precipitate is in equilibrium with the matrix solute concentration, Ce (Fig. 9.7a). Irradiation causes dissolution of the precipitate surface and an increase in the solute content near the interface that begins to diffuse away (Fig. 9.7b). Re-solution is balanced by re-precipitation and results in a steady state concentration profile (Fig. 9.7c). Local supersaturation of solute may lead to the nucleation of new precipitates in the matrix (Fig. 9.7d) or if the precipitates are very widely spaced, the matrix solute may not reach a value that results in steady state and the precipitate will continue to dissolve (Fig. 9.7e). Determining the stability of a phase under irradiation is complicated by the influence of multiple parameters such as the displacement rate, temperature, and sink strength. An estimate for the stability of a precipitate can be obtained by considering two opposing processes, ballistic mixing and radiation-enhanced interdiffusion. This problem was analyzed by Abromeit [13] and the analysis is summarized here. Precipitates are assumed to be dissolved by ballistic mixing at a rate approximated by: Rm = β σD φ ,

(9.21)

where the product of the displacement cross section, σD and the flux, φ is the displacement rate in dpa/s, and β is a factor that links displacement rate to solute loss from the precipitate. Similarly, the rate of formation or growth of a precipitate due to radiation-enhanced diffusion is given by: Rg = α D˜ ,

(9.22)

442

9 Phase Stability Under Irradiation Fig. 9.7. Schematic illustration of radiation-induced precipitate dissolution and precipitation as a function of dose. (a) Unirradiated state, (b) surface dissolution at low dose, (c) steady state, and either (d) nucleation of new precipitates due to local solute supersaturation in the matrix, or (e) continued dissolution of the precipitate due to low precipitate density (from [12])

where α is a constant and D˜ is the interdiffusion coefficient. The solubility limit may be determined by equating the two processes, yielding:

α D˜ = β σD φ .

(9.23)

The steady state point defect balance equations are written as in Chap. 5: K0 − KivCiCv − Dvks2Cv = 0 K0 − KivCiCv − Di ks2Ci = 0 ,

(9.24)

and the variables are as defined in Chap. 5, where Kiv = 4π rv Di /Ω , and ks2 = 4π rsCs /Ω is the sink strength. Note that in this analysis, no distinction is made in the sink strength for vacancies and interstitials. When recombination dominates defect loss: 1/2 1/2 D˜ = AK0 Dv (Ω /4π rv)1/2 ,

(9.25)

9.2 Recoil Dissolution

443

and when defect annihilation at sinks dominates, D˜ is temperature-independent and can be described as: D˜ = AK0 /ks2

(9.26)

and A is a constant describing the transport efficiencies of the atoms via vacancies and interstitials. Eliminating D˜ from Eqs. (9.25) and (9.26) defines the boundary between the regimes where recombination is dominant and where annihilation at sinks is dominant and gives: K0 = ks4 Dv (Ω /4π rv ) .

(9.27)

Equation (9.27) is shown by the plane, P1 in Fig. 9.8 that plots the solubility as a function of damage rate, temperature and sink strength. Given that σd φ = K0 /N the contribution of defect annihilation at sinks to the solubility limit is determined by eliminating D˜ between Eqs. (9.21) and (9.26) and yields the critical sink strength: kc2 = Aα N/β .

(9.28)

Equation (9.28) is shown as the plane, P2 in Fig. 9.8. Finally, according to Eqs. (9.23) and (9.25), a temperature-dependent boundary separates the two-phase from the one-phase regimes and is given as: K0 = (Aα N/β )2 Dv Ω /4π rv ,

(9.29)

Fig. 9.8. Stability diagram for precipitates under irradiation in displacement rate-temperaturesink strength space. The plane P1 separates recombination and annihilation regimes, and precipitates are stable below the plane P3 and to the left of the plane P2 (from [13])

444

9 Phase Stability Under Irradiation

and is shown as plane P3 in Fig. 9.8. Precipitates are stable below P3 and to the left of P2 . The region representing stability of the two-phase structure increases in size with increasing temperature due to increasing diffusivity and with increasing values of the critical sink strength, kc2 . The term β in Eq. (9.21) is approximated by β = β1Vc /Ω , where β1 is a constant and Vc is the volume of the collision cascade and is therefore proportional to the cube of the cascade radius, rc [13]. Re-precipitation of the solute dissolved into the matrix by the cascade is controlled by interdiffusion with the rate constant given by Fick’s law as α = 4α1 /rc2 , where α1 is a constant. Inserting these expressions for α and β into Eqs. (9.28) and (9.29) gives: 3π Aα1Ω N 1 , β1 rc5 Aα1 N 2 3Dv Ω 3 1 . K0 = β1 4π 3 rv rc10 kc2 =

(9.30) (9.31)

Note that both the critical sink strength and the production rate/temperature relationship exhibit a very strong dependence on the cascade size. The model was applied to the case of a Cu–48%Ni–8%Fe alloy irradiated with 300 keV Cu+ ions over a range of temperatures and displacement rates. Figure 9.9 plots the primary recoil rate vs. 1/T with the open symbols denoting irradiation-induced dissolution of the two-phase structure. Note that there is a critical displacement rate for irradiationinduced dissolution that increases with temperature. The line in the graph is the optimal fit of Eq. (9.31) to the data, from which the cascade radius was determined to be ∼ 2.7 nm. In summary, radiation-induced dissolution is a key process affecting the stability of precipitates. Radiation results in re-solution of the precipitate outer surface and

Fig. 9.9. Stability of the two-phase structure in Cu–48%Ni–8%Fe irradiated with 300 keV Cu++ . Filled symbols denote irradiation-induced disordering of the twophase structure and open symbols denote no irradiation effect. The line is the best fit of Eq. (9.31) (from [13])

9.3 Radiation Disordering

445

the evolution of the phase microstructure is then determined by the relative rates of re-solution and re-precipitation. In essence, phase stability is controlled by kinetic processes in the solid. Besides dissolution, precipitate stability is also affected by radiation-induced disordering, described in the next section.

9.3 Radiation Disordering The NHM model described in the last section was originally developed for both recoil dissolution and disordering dissolution. Disordering involves the loss of longrange order due to irradiation. In the case of disordering, displacement is assumed to occur in a shell of thickness, l at the precipitate surface and result in the loss of solute atoms by diffusion to the matrix. It is also assumed that only a fraction, f of these solute atoms actually become dissolved. Defining ξ = l f as the dissolution parameter, then the dissolution rate given in Eq. (9.1) becomes: dV = −4π rp2ξ K0 , dt

(9.32)

and the rate of change of the precipitate size due to disordering dissolution is: dr 3DC = −ξ K0 + − rp2 Dρ , dt 4π rpCp

(9.33)

which is identical to Eq. (9.6) except for the first term. Russell [14] points out that since l ∼ 10 nm, then for f ∼ 1, ξ = l f ∼ 10 nm. Comparing this value to the corresponding term in Eq. (9.6) for recoil dissolution, where ζ Ω ∼ 10−4 nm, shows that the disordering dissolution rate is much higher than that due to recoil dissolution, so disordering dissolution is expected to be a much more effective process. Referring back to Fig. 9.4 shows that the stable precipitate size will be lower for disordering dissolution due to its greater efficiency. Irradiation is known to disorder alloys by the creation of vacancies and interstitials and anti-site defects, in which the atoms are re-located to the complementary site, disrupting the order in the alloy. But disordered alloys will return to their equilibrium state as long as diffusion can occur. In fact, the high concentration of vacancies and interstitials produced by irradiation can enhance the ordering process by radiation-enhanced diffusion. Therefore, irradiation causes two opposing processes to occur: disordering and re-ordering. Liou and Wilkes [15] describe the rate of change of order in an alloy due to irradiation starting from the Bragg–Williams definition of long-range order for a binary alloy with atoms arranged on two sublattices, α and β , where the long-range order parameter is defined as: S=

( fAα − XA ) , (1 − XA )

(9.34)

where fAα is the probability of an A atom being on an α lattice site, and XA is the atomic fraction of A atoms. When S = 1, the alloy is completely ordered and when S = 0, the alloy is completely disordered.

446

9 Phase Stability Under Irradiation

Under irradiation, the rate of ordering can by written as a competition between radiation-induced disordering and thermal re-ordering: dS dS dS = + . (9.35) dt dt irr dt th The disordering rate due to irradiation can be written as: dS = −ε K0 S , dt irr

(9.36)

where ε is the disordering efficiency, or the ratio of replacements to displacements, and is of the order 10–100 under neutron irradiation. The thermal order-disorder transition can be written as a chemical reaction in which A and B atoms on the wrong lattice sites are interchanged so that the A–B pair is on the correct sites: Kc

(A − B)wrong (A − B)correct ,

(9.37)

Kw

where the rate constants, Kc and Kw are given by: Kc = νc exp(−U/kT ) , Kw = νw exp[(−U + VT)/kT ] ,

(9.38a) (9.38b)

where U is the energy barrier for the reaction and the activation energy, VT is the energy reduction when the wrong A–B pair transforms to the correct A–B pair and the νc,w are the frequency factors for the correct and wrong pairs, respectively. The solution of the chemical rate equations gives the following relation for the order parameter in terms of the equilibrium order parameter, Se and the time, t: (1 − S) = coth(kot + y) , (1 − Se)

(9.39)

where y is a constant and ko is the rate constant defined as: v i ko = νvCv exp(−Em0 /kT )(Zα + Zβ − 2) + νiσ Ci exp(−Em0 /kT ) (XA /XB )1/2 × Zβ exp(−V0 /2kT ) , (9.40) 1/2

1/2

where 2νv = (νc νw )v and 3νi = (νc νw )i are the frequency factors for exchange v and E i are the vacancy and interby vacancies and interstitials, respectively, Em0 m0 stitial migration energies for ordering, Zα is the number of α sites that are nearest neighbor to a β site and Zβ is the reverse, where α and β refer to the two sublattices, σ is a parameter accounting for the number of reaction paths and their probabilities and XA and XB are the atom fractions of A and B atoms, respectively. V0 is the activation energy for ordering, V0 = AV , where A is crystal structure dependent (A = 6

9.3 Radiation Disordering

447

for fcc and A = 14 for bcc) and V = VAB − (VAA +VBB)/2, where the VXY terms are the energies of the respective atom pairs. The time derivative of the thermal order parameter can be written as [15]: dS ko (1 − S)2 − (1 − Se)ko . = (9.41) dt th (1 − Se) The steady state solution to Eq. (9.35), where the terms are given in Eqs. (9.36) and (9.41), is: (1 − Se ) 2 2 4ko ε K0 1/2 S = 1 + ε K0 − ε K0 + 4ko2 + . (9.42) 2ko (1 − Se) Liou and Wilkes applied this formalism to the AuCu3 system as a function of temperature and dose rate. Figure 9.10 shows that at any given temperature, the effect of increasing dose rate is a reduction in the order, as expected. Also, for a given dose rate, increasing temperatures results in greater order. Another way of showing the competing effects of irradiation and temperature on the alloy order is given in Fig. 9.11a. Here, the equilibrium value of Se is 1.0, but the alloy is in a state where the order, Sobserved is less than Se . At low temperature, where defect motion is restricted, the effect of irradiation is to disorder the alloy. At high temperature, the effect of irradiation is to increase defect mobility so that the order parameter approaches equilibrium, which lies above the original, incompletely equilibrated state. That is, irradiation assists ordering at high temperatures. This behavior is further illustrated by the example shown in Fig. 9.11b, which is a first-order transition of a solid solution alloy in the disordered α phase to an ordered α phase. Under irradiation, the ordered phase becomes disordered at low temperatures, reverting to

Fig. 9.10. Steady state long-range order parameter for Cu3 Au under irradiation for various dose rates (from [15])

448

9 Phase Stability Under Irradiation Fig. 9.11. (a) Effect of irradiation on the temperature dependence of the order parameter for a phase structure that is not at the equilibrium order, Se . (b) Equilibrium phase diagram showing a first-order phase transformation of the disordered a phase to the ordered α -phase. (c) Modification of the phase diagram by irradiation reflecting the change in order as given in (a). (d) Dependence on the irradiationmodified phase diagram with dose rate (from [3])

the α phase as shown in Fig. 9.11c. Since the degree of disordering is dependent on the dose rate, the shape of the phase fields shown in Fig. 9.11c will change at higher dose rate. The dependence of the phase fields on dose rate is shown schematically in Fig. 9.11d, in which the ordered region continues to shrink with increasing dose rate. The change in the phase diagram caused by irradiation-induced disordering constitutes an irradiation modified phase transition as disordering can change the alloy phase structure. Recall that the ordered state is the arrangement of atoms that

9.3 Radiation Disordering

449

minimizes the free energy of the solid. Consequently, radiation-induced disorder increases the free energy of the solid above the equilibrium value. Hence, under irradiation, a new free energy balance may be achieved between adjacent phases in the alloy. Figure 9.12 shows how the compositions of the α and γ phases determined by the common tangent of free energy curves can be changed when irradiation induces an increase in the free energy of the intermetallic β phase, resulting in a partially disordered phase, β . Note that while the ordered β phase is in equilibrium with the α phase at a composition CA , partial disordering by irradiation raises the free energy of the β phase to β and the concentration of A in equilibrium with α and β phases is now CA . Further irradiation can lead to complete disordering, β phase, such that the phase does not form. Note that order-disorder transformation energies are generally in the range of 0.1 to 0.6 eV/atom [16]. The effect of irradiation on ordering can also be understood with the aid of the thermal spike model of the cascade, discussed in Sects. 3.3 and 10.2.4. Recall that the energy density in the core of the cascade can reach values such that the region resembles a liquid-like structure. Wollenberger [12] determined the time dependence of the temperature in the cascade as a function of the distance from the center of the spike, where temperature is normalized to the disordering temperature, Tc and the result is shown in Fig. 9.13 for nickel. In this figure, rc is the value of the cascade radius at which the temperature just reaches the disordering temperature at any time during the thermal spike, which in this case is 2.6 nm. As such, the temperature of the region inside this radius can be assumed to exceed Tc , resulting in disordering of the center of the cascade. Presumably, in the outer regions of the cascade where the temperature is below Tc but where the vacancy density is high, re-ordering will occur. In fact, when the re-ordered shell of a new cascade overlaps the disordered zone from an old cascade, the remaining disorder will be reduced, causing a reduction in the disordering efficiency per cascade with increasing fluence. The consequence of this overlap process is that the long-range order parameter will not completely vanish, even at high fluences.

Fig. 9.12. Schematic illustration of a phase diagram for an alloy with an ordered intermetallic compound, β showing partial disordering to β , and complete disordering, β due to the increase in free energy caused by irradiation (from [14])

450

9 Phase Stability Under Irradiation

Fig. 9.13. Time dependence of the temperature of a thermal spike for different radial locations within the spike (from [12])

At low temperatures where vacancies are immobile, irradiation-induced disordering can occur very quickly in some systems. For example, the γ phase (L12), NiAl3 , is extremely unstable under irradiation [17], becoming disordered following irradiation with 500 keV Kr at RT to a dose of 2 ×1014 i/cm2 [18]. On the other hand, Fe3 Al (bcc) and FeAl (bcc-B2) undergo only partial disordering after 40 dpa of 2.5 MeV Ni+ irradiation [19]. Hence, factors besides dose play a role in the orderdisorder transformation reaction in alloys.

9.4 Incoherent Precipitate Nucleation Irradiation can induce the formation of precipitates in an alloy. Precipitate growth and nucleation can be expressed as a chemical effect of vacancies and interstitials due to high levels of solute supersaturation under irradiation. The supersaturation provides the driving force for the reaction. Maydet and Russell [20] developed a model for the growth of spherical, incoherent precipitates under irradiation and that model is described here. The precipitate is characterized by two variables: the number of solute atoms, x and the number of excess vacancies, n, which is the difference in the number of matrix atoms displaced by the precipitate and x. Precipitates with greater atomic volume than the matrix must have n > 0 to relieve the strain energy, and undersized precipitates must have n < 0. The precipitate behavior is described by its movement in a phase space of coordinates n and x, much as was done with dislocation loops and voids in Chaps. 7 and 8. Figure 9.14 shows how the precipitate can move in phase space by capture of solute atoms, βx , vacancies, βv

9.4 Incoherent Precipitate Nucleation

451

Fig. 9.14. Precipitate trajectories in (n, x) phase space showing the processes giving rise to its motion (from [20])

or interstitials, βi , or the emission of solute atoms, αx or vacancies, αv . The particle moves in phase space with a velocity equal to the frequency of addition of solute or defect times the jump distance: x˙ = βx (n, x) − αx (n, x) ,

(9.43)

n˙ = βv (n, x) − αv (n, x) − βi (n, x) .

(9.44)

The β s are determined from concentrations and diffusivities of the defects and solute and the α s are determined as follows. As with void nucleation, there exists an energy barrier to the growth of the precipitate above some size, such that precipitates below this size equilibrate with each other and growth and shrinkage occur at the same rate. That is, the excess number of (n, x − 1)-mer gaining a solute atom to become a (n, x)-mer is balanced by the reverse process. The same holds for the number of (n − 1, x)-mer gaining a vacancy to become a (n, x)-mer. The equilibrium number of (n, x)-mer is then: ΔG0p (n, x) 1 0 , (9.45) ρp (n, x) = exp − Ωm kT where Ωm is the atomic volume of the matrix phase and ΔG0p (n, x) is the free energy of formation of a precipitate from n matrix vacancies and x solute atoms. The balance between (n, x − 1)-mer and (n, x)-mer can be written as:

βv (n − 1, x)ρp0(n − 1, x) = αv (n, x)ρp0 (n, x) ,

(9.46)

βx (n, x − 1)ρp0(n, x − 1) = αx (n, x)ρp0 (n, x) .

(9.47)

452

9 Phase Stability Under Irradiation

Substituting Eq. (9.45) into Eqs. (9.46) and (9.47) and replacing differences in ΔG0p (n, x) by derivatives, gives:

αv (n, x) ≈ βv (n, x) exp

αx (n, x) ≈ βx (n, x) exp

1 ∂ ΔG0p (n, x) kT ∂n 1 ∂ ΔG0p (n, x) kT ∂x

,

(9.48)

,

(9.49)

where βv (n − 1, x) and βx (n, x − 1) in Eqs. (9.46) and (9.47) vary slowly with n and x and have been replaced with their values at (n, x). The free energy change upon formation of a precipitate from a solid solution that contains a supersaturation of solute and vacancies is given as: ΔG0p = −nkT ln Sv + (36πΩ 2)1/3 γ x − xkT ln Sx +

Ω Ex(δ − n/x)2 , 9(1 − ν )

(9.50)

where Sv is the vacancy supersaturation, Sx is the solute supersaturation, Ω is the atomic volume of the precipitate, δ = (Ω − Ωm )/Ωm , γ is the matrix:precipitate surface energy, E is Young’s modulus, ν is Poisson’s ratio, and the remaining variables are as previously defined. The first two terms are the same as in the formation of a void from a supersaturation of vacancies given in Eq. (8.17) in which the first term is due to the vacancy supersaturation and the second term is the contribution of surface energy (with the number of solute atoms substituted for the number of vacancies in the aggregate). The third term reflects the effect of solute supersaturation, analogous to vacancy supersaturation, and the last term accounts for the elastic (volume) strain energy due to either an excess or deficit of vacancies from the stress-free condition (given by δ = n/x). Substituting into Eqs. (9.48) and (9.49) for αv (n, x) and αx (n, x) into Eqs. (9.43) and (9.44) gives: 1 ∂ ΔG0p , (9.51) x˙ = βx (n, x) − αx (n, x) = βx 1 − exp kT ∂ x 1 ∂ ΔG0p βi n˙ = βv (n, x) − αv (n, x) − βi (n, x) = βv 1 − − exp , (9.52) βv kT ∂ n where from Eq. (9.50) the arguments of the exponents are determined to be: 1 ∂ ΔG0p 2Ax−1/3 = − ln Sx + + B(δ 2 − n2/x2 ) , kT ∂ x 3 1 ∂ ΔG0p = − ln Sv − 2B(δ − n/x) , kT ∂ n with A =

ΩE (36πΩ 2 )1/3 γ and B = . kT 9kT (1 − ν )

(9.53) (9.54)

9.4 Incoherent Precipitate Nucleation

453

The behavior of the precipitate in (n, x) space may be described by constructing nodal lines in (n, x) space along which x˙ and n˙ individually are set equal to zero as follows:

βi 1 ln Sv 1 − , for n˙ = 0 , (9.55) n=x δ+ 2B βv

1/2 1 2A ln S n = xδ 1 + − , for x˙ = 0 . (9.56) x 3Bδ 2 x1/3 δ 2 B Figure 9.15 shows that the nodal lines in (n, x) space converge and cross at a critical point, beyond which they diverge. The critical point (n∗ , x∗ ) is found by solving Eqs. (9.55) and (9.56) simultaneously to obtain: 32πγ 3Ω 2 2γΩ , or rp∗ = − 3(Δφ )3 Δφ

β 1 i ln Sv 1 − n ∗ = x∗ δ + , 2B βv x∗ = −

where x∗ and rp∗ are related by x∗ = is given by:

(9.57) (9.58)

4/3π rp2 , and the irradiation-modified free energy Ω

Δφ = −kT ln Sx − δ kT ln[Sv (1 − βi/βv )] −

kT [ln Sv (1 − βi/βv )]2 . 4B

(9.59)

Figure 9.15 is constructed for the case where δ > 0, that is an excess of vacancies relative to solute. Under this condition, the region above the n˙ = 0 line contains an excess of vacancies and has a greater tendency for emission than capture, giving n˙ < 0, or shrinkage. The opposite is true for the x˙ = 0 nodal line in that the vacancy rich precipitate will increase its strain energy by solute emission, causing x˙ < 0 and

Fig. 9.15. Nodal lines, critical points and precipitate trajectories in (n, x) phase space for growth of an oversized, incoherent precipitate under irradiation (from [20])

454

9 Phase Stability Under Irradiation

supporting growth. As shown, particle growth is determined by the quadrants defined by the critical point. Precipitates grow in quadrant 1 and decay in quadrant 3 and behavior in quadrants 2 and 4 depend on the values of the capture terms. Precipitates that are between the nodal lines cannot escape. When with x > x∗ , precipitates will grow and when x < x∗ , they will decay. In general, irradiation will tend to stabilize a precipitate with δ > 0 and destabilize ones with δ < 0. Note that the unstable case of δ < 0 means that Δφ > 0, which can only occur if the first term in Eq. (9.59) is positive since the second term is always negative as long as βi /βv < 1. Physically, this means that since there is a net arrival of vacancies to the precipitate, those precipitates that need the vacancies to grow (e.g., an oversized precipitate, δ > 0) will be stabilized by irradiation. For an undersized precipitate phase (δ < 0) to grow from a slightly supersaturated solid solution without prohibitive strain energy, the particle must emit vacancies into the matrix. In the absence of excess vacancies, this is easily done, as vacancies arrive at and leave the interface at the same rate (in the absence of growth or decay), and there is no trouble in establishing a net flux tout to allow growth. Under irradiation, the vacancy emission rate is not altered, but the arrival rate is increased by several orders of magnitude. It is then almost impossible to achieve a net emission of vacancies. There will instead tend to be a net gain of solute atoms in the face of the slight solute supersaturation. The excess vacancies thus destabilize the undersized precipitate phase. The same arguments may be used to understand stabilization of an oversized precipitate. The potential function given in Eq. (9.59) has some of the properties of a free energy. It predicts whether precipitates of a given size will be stable under irradiation and provides the minimum stable precipitate size. In the absence of excess vacancies due to irradiation, Δφ in Eq. (9.59) becomes Δφ = −kT ln Sx , which is the Gibbs–Thompson equation. The effect of irradiation is to shift the effective free energy curve for the precipitate vertically by the amount δ kT ln[Sv (1 − βi /βv )]. If Δφ < 0, precipitates larger than x∗ will be stable, and if Δφ > 0, all precipitates will decay. Russell shows this schematically in Fig. 9.16. For this alloy, the θ phase is thermally stable and the ψ phase is not. The effect of irradiation is to destabilize the θ phase (δ < 0) and stabilize the ψ phase (δ > 0), by virtue of the sign of δ . Note that the order of stability is reversed by irradiation so that the θ phase would dissolve and the ψ phase would precipitate. The precipitation of the ψ phase under irradiation is an example of irradiation-induced precipitation in an undersaturated solid solution. The nucleation rate of precipitates due to irradiation can also be estimated. The nucleation rate is the number of precipitate nuclei growing past a certain value of x per unit time and volume [22]. At steady state, the nucleation flux is independent of x, and the nucleation rate can be given at an arbitrary value of x as: Jp (x) =

∞

∑

[βx (x)ρp (n, x) − αx (n, x)ρp (n, x + 1)] ,

(9.60)

n=−∞

and the summation converges rapidly for large values of n due to the effect of strain energy. Figure 9.17 shows how the nucleation rate varies with supersaturation of

9.5 Coherent Precipitate Nucleation

455

Fig. 9.16. Schematic phase diagram showing the effect of irradiation on the stability of incoherent precipitates in the case where the precipitate is thermally stable (θ ) and thermally unstable (ψ ) (from [21])

vacancies and solute in the Al–2%Ge system under irradiation. As expected, the nucleation rate increases with both Sx and Sv , but is more sensitive to Sx . Figure 9.17a shows the huge effect of excess vacancies alone on precipitate nucleation. Excess vacancies elevate the nucleation rate from infinitesimal to a high value giving a high precipitate density. Figure 9.17b shows that the effect of excess interstitials is to reduce the nucleation rate somewhat, but by factors small compared to the huge enhancements due to the vacancies. Irradiation is thus a tool for creating phases which otherwise might be impossible to obtain, and also for preventing the formation of phases that are otherwise stable.

9.5 Coherent Precipitate Nucleation The preceding analysis applies for the precipitation of incoherent precipitates from a solid solution due to irradiation. We consider here the precipitation of coherent precipitates due to irradiation. The distinction between these two cases lies in the behavior of point defects at the precipitate surface. As shown in Chap. 8, incoherent precipitates behave like voids in that defects can be absorbed and emitted. However, the coherent precipitate interface acts as a defect trap such that the defect retains its identity. This feature has the result of reducing the problem of determining the energy change due to precipitation from a two-dimensional (n, x) problem to a one-dimensional (x) problem. Cauvin and Martin [23], as summarized by Russell [14] described the pseudo-equilibrium precipitate size distribution under irradi-

456

9 Phase Stability Under Irradiation

Fig. 9.17. (a) Dependence of nucleation rate on solute supersaturation for various vacancy supersaturation levels, based on a solid solution of Ge in Al at 23 ◦C. (b) Effect of interstitial– vacancy arrival rate ratio on the nucleation rate for several solute and vacancy supersaturation levels, based on a solid solution of Ge in Al at 123 ◦C (from [21])

ation, ρ (x) as:

ρ (x) ρ 0 (x) = B(x) , ρ (x + 1) ρ 0 (x + 1)

(9.61)

9.5 Coherent Precipitate Nucleation

457

where ρ 0 (x) is the equilibrium size distribution in the absence of irradiation produced defects and B(x) is defined by: B(x) =

βv (x)[ρv (x) + ρn(x)] + βi (x)[ρi (x) + ρn(x)] , [βv (x) + βi (x)]ρt (x)

(9.62)

where: ρi (x) = number of clusters with trapped interstitials ρv (x) = number of clusters with trapped vacancies ρn (x) = number of clusters with no trapped defects, ρt (x) = ρi (x) + ρv (x) + ρn(x) . The quantity B(x) is the fraction of solute arriving at the precipitate that does not result in defect annihilation. The thermal and irradiation-modified solubilities are related by: Cirr = C0 B(∞). In parallel with the equilibrium free energy, the pseudo-free energy, ΔG (x) is given in terms of the pseudo-equilibrium precipitate size distribution, ρ (x) as: 1 ∂ ΔG ρ (x) = exp . (9.63) ρ (x + 1) kT ∂ x As with an unirradiated solid solution in which a metastable condition exists if G(x) has a maximum in x, then G (x) must have a maximum in x for metastability in the irradiated state. Recalling that ρ 0 (x) = exp(−G0 (x)/kT ), then Eq. (9.61) can be rewritten using Eq. (9.63) as:

∂ G (x) ∂ ΔG0 (x) = + kT ln B(x) , ∂x ∂x

(9.64)

and B(x) has one of two forms depending on the sign of the term, σ defined as:

σ=

(1 − pi/pv ) . (1 − βi/βv )

(9.65)

where pi,v is the probability of a particular trapping site being occupied by an interstitial or a vacancy. For either case, the value of B approaches a constant with increasing values of x, and in similar fashion for large x:

∂ ΔG0 (x) = −kT ln Sx , ∂x

(9.66)

and Eq. (9.64) can be written as:

∂ G (x) = −kT ln Sx + kT ln B(x) . ∂x

(9.67)

Figure 9.18 shows the terms of the expression in Eq. (9.64) for the pseudo-free energy of the solid solution under irradiation for various values of σ . When σ < 0, if −kT ln B(∞) > −kT ln Sx , then the solution will be metastable, as in Fig. 9.18a. If

458

9 Phase Stability Under Irradiation

Fig. 9.18. Schematic illustration of stability altered by defect recombination at the particlematrix interface. (a) σ < 0, 1 root. (b) σ > 0, 1 root. (c) σ > 0, 2 roots (from [23]). (d) Dose rate-temperature dependence of precipitation of Ni3 Si, γ from undersaturated Ni–Si solid solution alloys irradiated with 1 MeV electrons, – Ni–6at%Si, Ni–4at%Si, – Ni–2at%Si. (e) Increase in temperature at which Zn rich clusters, or G.P. zones are stable with increasing irradiation dose rate by 1 MeV electrons over a range of Zn concentration in the Al–Zn phase diagram. Half circles to the right (left) indicate data at high (low) irradiation flux. Full (open) symbols indicated occurrence (absence) of irradiation-induced precipitation. Dashed line is the stability limit in the absence of irradiation (from [24])

∂ G (x) = 0 may have 0, 1 or 2 roots. The solid solution is σ > 0, then the solution to ∂x stable if there are 0 roots. With one root, the solution is metastable (Fig. 9.18b). But in the case of 2 roots (Fig. 9.18c) the solution is metastable below the value x∗∗ , and the precipitate could never grow to large size. Note that in this model, irradiation will always decrease solid solubility.

9.5 Coherent Precipitate Nucleation

459

Table 9.1. Irradiation-induced precipitation in undersaturated binary alloys (from [24]) Alloy

Projectile

Precipitate

Morphology

MgCd AlZn

e− n e− e− Ni+ e−

Mg3 Cd β Zn G.P. zones and β Zn (100) Ag-rich platelets β NiBe β NiBe

NiSi

n Ni+ e− H+

γ γ γ γ

NiGe CuBe

e− e− Cu+ Cu+ H+ H+ N+ e− n e− e− n, ions, e−

γ Ni3 Ge G.P. zones γ Mo γ Pd3 Fe bcc W WRe3 , W-Re unidentified “ changes of composition

– homogeneous precipitation homogeneous precipitation homogeneous precipitation at interstitial dislocation loops homogeneous precipitation and at interstitial dislocation loops at interstitial dislocation loops “ “ coherent, triggered by inhomogenity of defect production at cavities and dislocation lines homogeneous precipitation at cascades at dislocation loops at dislocation loops at dislocation loop s homogeneous precipitation homogeneous precipitation “ –

AlAg NiBe

PdMo PdFe PdW WRe FeV FeCr various ternaries

Ni3 Si Ni3 Si Ni3 Si Ni3 Si

A compilation of precipitates formed in undersaturated solid solutions due to irradiation is shown in Table 9.1. Note that precipitation can occur with many particle types and over large ranges of temperature and dose rate. The relation between these latter two variables is important and is highlighted in Figs. 9.18d,e. Figure 9.18d is constructed from 1 MeV irradiation of several undersaturated Ni–Si solid solution alloys and delineates the region of Ni3 Si, γ precipitation from the solid solution, as shown by the filled circles. Figure 9.18e shows the dose dependence of solubility in Al–Zn. With increasing dose rate, formation of Guinier-Preston (GP) zones (Zn-rich clusters) in Al–Zn occurs at higher temperatures compared to the stability limit in the absence of irradiation (dashed line). Both of these examples show that irradiation of an undersaturated solid solution can lead to precipitation under irradiation at temperatures where the precipitate would not be thermally stable. They also underscore the strong coupling between temperature and dose rate in irradiation-induced precipitation. In summary, irradiation can affect phase stability by numerous processes: solute enrichment or depletion, precipitate re-solution, precipitate disordering, and irradiation-induced nucleation of both incoherent and coherent precipitates. Irra-

460

9 Phase Stability Under Irradiation

diation can also induce the formation of phases that are not stable under equilibrium conditions or metastable phases. Metastable phase formation is discussed in the next section.

9.6 Metastable Phases Since the term metastable implies a phase with a free energy higher than that of the stable phase under the prevailing conditions of temperature and pressure, it is natural to look to thermodynamics to explain their formation under irradiation. Experimental results seem to indicate a strong role of thermodynamics in the tendency to form metastable phases. Intermetallic compounds with small ranges of solubility and complex crystal structures are prime candidates for transformation to a metastable phase [19]. Also, the change in the free energy of the solid due to irradiation-induced defect buildup argues for a thermodynamic explanation [25]. However, not all transformations can be explained on a purely thermodynamic basis as solids under irradiation are generally far from equilibrium. Irradiation can be considered as similar to a quench process in which the atom configurations are essentially determined during the relaxation period following the collision events. At low temperatures, kinetics are restricted and the formation of complex crystalline structures is unlikely. Irradiation will usually result in solid solution, simple cubic structures or amorphous structures. The structure of the metastable system is, however, influenced by the equilibrium nature of the system. Those systems with many intermetallic compounds will form amorphous phases while those with no intermetallic alloys show a tendency to form solid solutions. At high temperature where atom mobility is significant, equilibrium phases will usually form. Metastable phases can be formed by neutron irradiation or by ion irradiation, ion implantation and ion beam mixing. Differences in the transformation process between ion irradiation techniques can provide insight into the mechanism governing metastable phase formation. For example, in ion irradiation experiments, the main result of the radiation is imparting damage to the lattice. However, in ion implantation, the implanted species provides a chemical alteration to the target as well. Ion beam mixing experiments are designed to follow the transformation by rapidly (far from equilibrium) altering the bulk content of the film. Metastable phases formed by irradiation usually occur by one of four types of transformations [26]: order → disorder crystal structure transformation: A → B crystal structure A → quasicrystal structure crystal structure A → amorphous structure The first three transformations will be briefly discussed and amorphization will be discussed in Sect. 9.7. For a more complete discussion of metastable phase formation, the reader is referred to [27].

9.6 Metastable Phases

461

9.6.1 Order–Disorder Transformations The order-disorder transformation and its role in phase stability was discussed in Sect. 9.3. However, radiation-induced disorder has been linked to metastable phase formation. In fact, many compounds are believed to undergo chemical disordering prior to amorphization under electron irradiation. Luzzi and Meshii [28] showed that of 32 compounds irradiated, all underwent chemical disordering and 15 amorphized. They concluded that irradiation-induced chemical disordering provided the driving force for amorphization, and cited the difficulty in forming the amorphous structure in pure metals as support for this argument. The linkage between disordering and amorphization also depends on the irradiation conditions, in particular the mass of the particle and whether damage is introduced via Frenkel pairs (electron irradiation) or in cascades (heavy ion irradiation). Comparison of the enthalpy for the order-disorder transformation to that for the crystalline-to-amorphous transformation shows that ΔHO-D ∼ 5ΔHc-a [16]. So in fact, the enthalpy change for disordering may be sufficient to induce amorphization. The role of disordering in the onset of amorphization will be discussed in Sect. 9.7. 9.6.2 Crystal Structure Transformations Numerous examples exist on the transformation from one crystal structure to another upon ion irradiation. One of the simplest examples is the transformation of pure nickel metal from fcc to hcp under irradiation. This transformation has been found to occur during irradiation with a variety of species including neutrons, chemically inert elements such as He and Ar, the metalloids P and As, as well as selfirradiation [29]. Observations on P-implanted high purity Ni [30] revealed an orientation relationship between the new hcp phase and the fcc matrix similar to that observed for martenistic fcc → hcp transformations. The transformation in Ni is thus believed to be martensitic. TEM examination of Sb-implanted Ni showed hcp particles extending 20 nm beyond the implanted depth, but dechanneling is present up to 130 nm, suggesting that the defect distribution is playing a role in the structure transformation. Ion irradiation has also been found to induce phase transformations between bcc and fcc phases in iron-based austenitic alloys [31]. The most prominent example is the fcc-to-bcc transformation of 304 stainless steel following implantation with 3 ×1016 Fe+ /cm2 at 160 keV. Although this dose amounted to an increase in the Fe alloy composition by only ∼ 1 at% (67 at% Fe nominal), the structure transformed from fcc → bcc. The orientation relationship was neither the Kurdjumov–Sachs nor the Nishijima–Wasserman relationships typically found in ion-irradiated steels [31], but instead obeyed the following relationship: (100)bcc ||(100)fcc

and [010]bcc ||[011]fcc .

(9.68)

Follstaedt [32] suggested that the transformation need not be occurring martensitically, but that the increased defect concentration and hence, diffusivity, may be responsible for the transformation. It should also be noted that this transformation is

462

9 Phase Stability Under Irradiation Fig. 9.19. Irradiationinduced solid solubilities for binary metal systems of positive heats of formation (from [33])

fundamentally different from that of nickel under irradiation in that the transformation is from the metastable state to the equilibrium structure, whereas in the case of Ni, the transformation is from the equilibrium fcc structure to a metastable hcp structure. The heat of formation of an alloy can have a strong influence on whether a metastable phase forms. Figure 9.19 shows the irradiation-induced solubilities for several binary metal systems as a function of the heat of formation, ΔHf . The samples were in the form of multilayers and were bombarded at 77 K by 400 keV Kr+ ions. All systems had positive values of ΔHf , meaning that in thermal equilibrium there is no, or only a limited miscibility of the components of the considered system. Note that the data points of the systems whose components have the same structures and of systems with components of different structure follow smooth curves. Both curves exhibit a rapid decrease from complete solubility to levels below 15 at% in a range of ΔHf of about 12 kJ/mol. However, even at large values of ΔHf , the solubility still has not disappeared. Metastable solid solutions can also form by displacement mixing at temperatures at which radiation-enhanced diffusion is sufficiently slow to maintain the supersaturated solid solution phase. Ion beam mixing of multilayered Ag–Cu targets form a continuous series of metastable solid solutions across the phase diagram. Although the phase diagram of the Cu–Ag system is a simple eutectic one with rather small solubilities of Ag in Cu and Cu in Ag, irradiation produced a single phase, metastable solid solution with the fcc structure across the entire Cu–Ag system [34]. Since ion beam mixing takes place mainly in the solid state, extended solid solutions can be achieved in nearly immiscible systems such as Ag–Ni. Even in the binary Au–Fe and Au–V systems which have more complex phase diagrams exhibiting a large solubility gap and several intermetallic compounds, respectively, and the bcc structure at the Fe– and V-rich terminal solid solutions, metastable solid solu-

9.7 Amorphization

463

tions form across both systems during ion beam mixing [35]. In all cases, the lattice parameters of the solid solutions vary smoothly with composition and show small or moderate deviations from Vegard’s law between the appropriate end-members. 9.6.3 Quasicrystal Formation The most novel metastable phases are the quasicrystalline phases, produced by ion irradiation of specific Al alloys. These phases show long-range order, but possess forbidden crystalline symmetries such a five or sixfold symmetry. The phase was discovered by Shectman et al. [36] at the National Bureau of Standards. Quasicrystals have positional order, but are neither periodically nor randomly spaced; instead, they are quasiperiodically spaced. This means that, given the position of one unit cell, the positions of the other unit cells are determined according to a predictable but subtle sequence that never quite repeats. Because these structures are highly ordered like crystals but are quasiperiodic instead of periodic, they have been called quasiperiodic crystals, or quasicrystals for short. The first quasicrystals formed by ion irradiation were in the Al–Mn system and examples extend into ternary and quaternary systems as well. In these initial experiments, the quasicrystal phase was formed by irradiating alternating layers of Al and Mn in the composition Al84 Mn16 with 400 keV Xe ions to doses of 2 – 10 ×1015 Xe/cm2 at 80 ◦C [37, 38]. Results showed that the icosahedral phase forms without a separate thermal treatment at or above 80 ◦C while the amorphous phase forms at 60 ◦C. The icosahedron is a regular polyhedron possessing twenty identical triangular faces, thirty edges and twelve vertices. The black pentagons on the surface of a soccer ball are centered on the vertices of an icosahedron. This observed dependence on sample temperature suggests that the icosahedral phase does not form within the dense ion cascade, but rather during subsequent defect evolution. Similar results have been achieved with freestanding Al–Fe multilayered samples [39], indicating that both multilayered and amorphous samples can be transformed to the quasicrystalline phase. In addition to temperature, the composition of the samples has an important effect on quasicrystal formation, establishing that quasicrystals are formed within a well-defined composition and temperature region.

9.7 Amorphization Irradiation can induce the formation of amorphous phases in alloys. Although the phase space available to an alloy is extremely large, only one point corresponds to an absolute minimum in free energy. This point represents the equilibrium phase. Given sufficient time, at any temperature greater than zero, the system will find that point and settle into the equilibrium phase. Nonetheless, there are generally other minima in the free energy phase space, which are of varying depths. These other minima correspond to metastable phases. Certain of these phases exhibit compositional short-range order (CSRO) very similar to that of the equilibrium phase but with different compositional long-range order. Similarly, the spatial arrangements

464

9 Phase Stability Under Irradiation

of the atoms on a small scale (topological short-range order, TSRO) can be very similar to the equilibrium phase but with different long-range order (such as fcc vs. hcp phases). In general, there may exist many phases with CSRO and TSRO that are nearly identical to the equilibrium phase. Common examples of such metastable phases include glasses and crystalline solids with a slightly different unit cell than the equilibrium. It has been suggested that in alloys with large negative heats of formation, disruption of chemical short-range order will lead to lattice destabilization and the formation of an amorphous phase [40]. In fact, the data on ion irradiation of intermetallic compounds supports just this sort of conclusion [22, 40]. Contradicting these observations are results of electron irradiation that show that complete longrange disordering often precedes the formation of an amorphous phase [26, 41]. For intermetallic compounds such as NiAl or FeTi, electron irradiation disorders but does not amorphize the compounds [42]. Irradiation with light ions produces much the same result as electron irradiation in that the amorphous phase is difficult to form, suggesting that disruption of CSRO is not adequate for lattice destabilization and that another mechanism must be responsible for amorphization such as topological disorder [42, 43, 44, 45, 46]. In fact, self-ion irradiation of Ni that induces a phase change from stable fcc to metastable hcp as discussed in Sect. 9.6, clearly has no chemical component and must be a result of the topological disorder introduced into the system by the Ni+ beam. The next two sections discuss the roles of heat of compound formation, crystal structure differences, solubility range of intermetallic compounds and the critical defect density on the formation of the amorphous phase. 9.7.1 Heat of Compound Formation and Crystal Structure Differences A good correlation exists between the heat of formation of a compound and the formation of amorphous phases in metal–metal systems [47], with large negative heats of formation tending to amorphize under irradiation. A plot of the ratio of the atomic radii vs. the heat of formation calculated using the Miedema model [48] shows where amorphization will occur (Fig. 9.20). In fact, alloys do not become amorphous if the heat of formation is greater than about +10 kJ/mol. However, the amorphous structure can be formed by ion mixing if the heat of formation is higher, e.g., Cr/Ag, Co/Cu, Fe/Cu and Co/Au. Specific compositions in the Au–Ir, Au–Ru and Au–Os systems, whose heats of formation range from +19 to +27 kJ/mol, were made amorphous by irradiation [33]. It has also been observed that crystalline phases of simple structures such as solid solutions or simple cubic structures form under irradiation, while amorphous phases are formed from more complex structures. This is explained by the short duration of the relaxation stage following the thermal spike. During the relaxation period, atoms attempt to re-arrange themselves. If the relaxation time is sufficient for precipitates to nucleate, crystalline phase formation may be achieved. The time required for nucleation is strongly influenced by the temperature, the crystalline structure of nuclei and the composition of the films that have been homogenized

9.7 Amorphization

465

Fig. 9.20. Ratio of atomic radii vs. the heat of formation of an equiatomic compound ( metal-metal crystalline, metal-metal amorphous, ◦ metal-metalloid crystalline, • metalmetalloid amorphous) (from [47])

with thermal treatments or ion beams. If the overall composition is not close to a simple crystal structure in the equilibrium phase diagram and there is not a strong chemical driving force (as well as mobility) to promote significant atomic motion, then crystalline phase formation may be inhibited. The role of structure difference in the propensity for irradiation-induced amorphization can be understood with the aid of a binary constitution diagram of an A–B alloy (Fig. 9.21a) a schematic free energy diagram for this alloy (Fig. 9.21b) and the corresponding polymorphic phase diagram (Fig. 9.21c) [49]. Note that the T0 curves in Fig. 9.21c are obtained from the crossing of the solid free energy curve with that of the liquid (or amorphous) curve at a given temperature. The T0α line defines the thermodynamic composition limits of the α -solution. When the concentration profile induced by mixing falls locally outside these limits, the α -solution is superheated with respect to the liquid (amorphous) phase and is not stable. Since melting is a local phenomenon not involving long-range diffusion, and since solids are not observed to withstand extensive superheating, it follows that observation of an α phase outside these composition limits represents an unstable state. Such a state will likely melt or amorphize before thermal spike evolution is complete. This leads to the first fundamental rule for solid phase formation. Johnson et al. [49] suggest that terminal solid solutions α and β can be formed up to the limits of the T0α and T0β curves (i.e., within the polymorphic phase diagram limits of α and β ). Solutions formed outside these limits are superheated and unstable against amorphization or melting. Secondly, intermetallic compounds with broad equilibrium homogeneity ranges (wide polymorphic limits in Fig. 9.21), and

466

9 Phase Stability Under Irradiation Fig. 9.21. (a) Binary constitution diagram of an A– B alloy. (b) Schematic free energy diagram for the alloy at temperature T2 . (c) Polymorphic phase diagram corresponding to the equilibrium phase diagram in part (a). The dashed lines show part of the original equilibrium diagram. Solid lines are representative T0 lines of each phase. The T0 lines define regions of polymorphic solid formation from the liquid state. Regions outside correspond to liquid or amorphous (polymorphic) states (from [49])

low-energy interfaces with α -solution or β -solution phases, may form in the prompt cascade provided that their respective growth kinetics allow high growth velocities. Compounds with narrow homogeneity range and complex chemically ordered unit cells should not form. Finally, amorphous phases are expected whenever the ion induced composition profile CB (z) lies outside the polymorphic limits of crystalline

9.7 Amorphization

467

Fig. 9.22. Possible configurations of an equilibrium, twophase alloy under irradiation at temperature T . Irradiation to an effective temperature, T1 gives amorphous and crystalline phases of different composition, while more intense irradiation to an effective temperature, T2 gives a single uniform amorphous phase (from [59])

phases. Amorphization may occur in addition when polymorphic limits permit compound formation but kinetics of compound formation or growth are slow. Martin [50] proposed a theory for amorphization that is similar in nature to that of Johnson. In this model, he adds the ballistic radiation recoil re-solution displacement jumps to thermally activated jumps to obtain an irradiation-altered diffusion equation. The practical effect of irradiation is then to cause the system to assume the configuration at temperature T that would be stable at a temperature T in the absence of irradiation: T = T (1 + DB /D ), where D is the thermally activated diffusion coefficient and DB is the diffusion coefficient including ballistic effects (Fig. 9.22). The theory predicts that irradiation of an equilibrium alloy of two solid phases at temperature T could raise the effective temperature to T1 , or under sufficiently intense irradiation to T2 . At T1 the irradiated alloy would at steady state be composed of amorphous and crystalline phases of different compositions. Irradiation intense enough to raise the effective temperature to T2 would produce a uniform amorphous alloy. 9.7.2 Solubility Range of Compounds and Critical Defect Density The tendency toward amorphization of the intermetallic compounds by irradiation correlates reasonably well with the degree of solubility within the phases. That is, alloys with limited solubility or a narrow compositional range show greater tendency for amorphous transformation. This correlation is also consistent with the concept that a critical energy or defect density must be created before the amorphous transformation can occur. If the total free energy of the defect crystalline state becomes greater than that of the amorphous state, a spontaneous transformation should occur. Associated with this critical free energy is a critical defect concentration. If this critical defect concentration can be reached under irradiation, then the crystal should

468

9 Phase Stability Under Irradiation

relax into the lower free energy (amorphous) state. This critical defect concentration has been estimated at 0.02 for silicon and germanium [51]. An estimate of the defect concentration required for amorphization can be made based on the increase in energy of lattice upon formation of a stable Frenkel pair. Each Frenkel pair will raise the energy of the alloy by an amount equal to the enthalpy of defect formation, ΔHi-v . The concentration of vacancy–interstitial pairs, Ci-v needed to increase the energy of the alloy by ΔHc-a can be estimated from the relationship: ΔHc-a = Ci-v ΔHi-v .

(9.69)

The magnitude of ΔHi-v for an fcc metal is approximately 5 eV, and ΔHc-a is approximately 0.06 eV/atom [16], giving the critical vacancy–interstitial concentration for amorphization as ∼ 0.01. However, such levels are not possible at reactor core component temperatures, but may be achievable in laboratory experiments conducted at temperatures where vacancies are immobile. The link between defect density and degree of solubility can be understood by referring to the free energy diagram in Fig. 9.23. Compounds with no or limited compositional range will undergo a greater increase in free energy than those with wide compositional range. The greater increase in free energy is due to the inability of the compound to exist in equilibrium outside the designated composition range. This is manifest in the narrow and steeply rising free energy vs. composition curves. For ordered phases (intermetallics) the increase is not only due to point defects, but anti-site defects in regions of localized non-stoichiometry. This proposed solubility rule is very consistent with Johnson’s thermodynamic analysis [49]. Note that for NiAl3 , only a slight deviation from stoichiometry is needed to result in a very large rise in the free energy. Therefore, the critical anti-site defect density would be low for NiAl3 as compared to NiAl. Anti-site defects may play a critical role in the amorphization process since calculations have shown that the critical defect density may be difficult to reach accounting for only point defects. However, since the defect concentration is strongly dependent on atom mobility and this is largely unknown in intermetallic compounds, accurate estimates of defect concentration are difficult to determine. Further, the critical defect density will be strongly temperature-dependent with higher concentrations required at higher temperatures. Further support for the existence of a critical defect density is provided by the observation that compounds that become amorphous during irradiation do not show evidence of prior dislocation loop formation [25, 52]. Although it has been assumed that the attainment of a critical defect concentration will cause an amorphous transformation, the high free energy associated with the point defects can also be relieved through the formation of a dislocation structure through the collapse of interstitial or vacancy clusters into small loops. However, observations show that either a material transforms directly to the amorphous state or forms dislocation loops. Since greater mobility is required for the formation of dislocation loops, and the maximum defect concentration associated with the nucleation of loops in irradiated metals is ∼ 10−4 [53], almost two orders of magnitude less than that for amorphization, indicates that defect mobility is a key factor in the amorphization process. This

9.7 Amorphization

469

Fig. 9.23. Ni–Al phase diagram (a) with hypothetical free energy diagram (b) at the irradiation temperature (from [19])

observation is consistent with the ease of amorphization in intermetallics where defect mobility is low, and the preferential formation of dislocation loops in pure metals and solid solution alloys where the mobility is high.

470

9 Phase Stability Under Irradiation

9.7.3 Thermodynamics and Kinetics of Amorphization In many respects, the C → A (crystalline-to-amorphous) transformation can be understood by relating it to melting by virtue of the similarity of these transformations. For example, amorphization is known to occur in a heterogeneous manner, similar to the first-order nucleation and growth process characteristic of melting. Also, Brillouin scattering studies have shown that intermetallics undergo a softening in the shear modulus, analogous to that observed at the onset of melting of many metals. As such, the C → A transformation can be considered to be a type of melting transformation. Okamoto et al. [54] wrote a comprehensive review of the physics of the crystalline-to-amorphous phase transformation. The role of irradiation in this transformation as presented in their paper is followed here. The liquid to glass transition is characterized by a temperature called the glass transition temperature, Tg . The glass transition is not a thermodynamic phase transition, but rather the point in the relaxation process where configurational equilibrium can no longer be achieved during the experiment. In this regard, it is more of a kinetic parameter that depends on the time-scale of observation. Free energy plots of the glass transition for perfect and defected crystals are shown in Fig. 9.24. The perfect crystal is shown by the bottom line and the defected crystals, denoted by the dashed lines, have higher free energies. The melting temperatures are given by Tm0 and Tmd , respectively. Also shown are two glass transition temperatures, Tg corresponding to an unrelaxed glassy state and Tk corresponding to the ideal glass

Fig. 9.24. Schematic plot of the Gibbs free energy as a function of temperature for a perfect crystal, the liquid phase and two defective crystalline states. Tm0 and Tmd are the thermodynamic melting temperatures of the perfect and defective crystals, respectively, Tg is the kinetic glass-transition temperature for the unrelaxed glassy phase and Tk is the ideal glass transition temperature (from [54])

9.7 Amorphization

471

transition temperature. Since the glass transition temperature is dependent on time, it is postulated that there exists some temperature, Tk below which the transition will never occur, and is known as the ideal glass temperature. Note that these points lie at a higher free energy than that of either the perfect crystal or the defected crystal. As described by Okamoto et al. [54], one of the simplest models of melting is due to Lindemann [55] who proposed that crystals melt when the root-mean-square + 2 ,1/2 of atoms from their equilibrium sites becomes (rms) thermal displacement, δvib large enough to encroach on nearest neighbors, or when the vibrational amplitude + 2 ,1/2 /rnn is about 50% of the interatomic spacing. Thus, melting occurs when δvib + 2 ,1/2 reaches a critical value equal to some fraction δcrit /rnn of the nearest neighbor spacing, rnn . In the harmonic Debye model of crystal lattices, the mean square thermal displacement for a perfect crystal at a temperature T above the Debye temperature, Θ0 is: + 2 , 36π 2 h¯ 2 T δvib = , MkΘ02

(9.70)

where h¯ is Planck’s constant, + k2 is, Boltzmann’s constant and M is the atomic mass. Since melting occurs when δvib reaches some critical value. Then from Eq. (9.70) the melting temperature of the perfect crystal is: Tm0 =

MkΘ02 + 2 , δcrit . 36π 2 h¯ 2

(9.71)

+ 2 , The + 2 total , mean-square atomic displacement is composed of thermal δvib and static δstat components, where the latter is due to defect structures such as point defects, anti-site defects, size mismatch between solute, solvent atoms in solid solution, defect clusters and impurities. The generalized form of the Lindemann melting criterion then becomes: + 2 , + 2 , + 2 , (9.72) δcrit = δstat + δvib , + 2 , where δcrit is a constant. Referring back to Fig. 9.24, this criterion , that + 2 the , + shows 0 2 crystal can be melted either by heating it to the melting + 2 , point, Tm ( δvib = δcrit ) or by increasing the amount of static disorder, δstat in the crystal until the free energy is equal to that of the liquid. As the damage level increases, the melting temperature of the defective crystal, Tmd defined by the intersection of the free energy curve with that of the supercooled liquid, decreases, as shown in Fig. 9.24. The maximum damage state will occur when the free energy curve of the defective crystal is tangent to that of the supercooled liquid, shown as the upper most dashed line in Fig. 9.24. + 2 , + 2 , = δcrit , or where Tmd = 0, is the theoretiThe state of maximum damage, δvib cal upper limit for damage accumulation in a defective crystal. , 9.25 shows + Figure 2 represents the a polymorphous melting curve for a defective crystal in which δstat

472

9 Phase Stability Under Irradiation

sum total of the effect of all defects in the crystal. The linear region follows from Eq. (9.72). Along the melting curve, where T = Tmd , Eq. (9.72) becomes: + 2 , + 2 , 36π 2h¯ 2 Tmd δcrit = δstat + , MkΘ02

(9.73)

which is written in the form of Eq. (9.71) as: Tmd =

MkΘ02 + 2 , δcrit , 36π 2 h¯ 2

where the Debye temperature of the defective crystal, Θ d is given as: + 2 , δ 2 2 , . Θd = Θ0 1 − + stat 2 δcrit

(9.74)

(9.75)

+ 2 , → 0, Θd2 → Θ02 , and Tmd → T0d . Note that Eq. (9.74) shows In a perfect crystal, δstat + 2 , that the proportionality between the melting temperature and δstat , Fig. 9.25, is related to the Debye temperature given in Eq. (9.75). Also, since Θd2 is proportional to the shear modulus, μd , the linear decrease in melting temperature also means that disorder-induced reduction + 2 , of the shear modulus is occurring with . From these proportionalities, we can the same functional dependence on δstat

Fig. 9.25. Generalized + 2disorder + 2 , T0 curve showing schematically the effects of static atomic , as measured by δstat , on the melting temperature of the defective crystal, Tmd . δmax and + 2 , + 2 , δcrit are the critical values of δstat for thermodynamic and mechanical melting (from [54])

9.7 Amorphization

write: Tmd μd Θd2 = = = 0 Tm μ0 Θ02

+ 2 , δ , . 1 − + stat 2 δcrit

473

(9.76)

If it were possible to relate the defects created by irradiation to the mean square displacement in the solid, then we could use Eq. (9.76) to determine the amorphization criterion directly. Since this is not possible, there are two alternative ways of determining the amorphization criteria. One is through disordering and another is through free energy change. Radiation-Induced Amorphization Driven by Disordering Recall that in Sect. 9.6 we determined that the disordering energy should be sufficient to drive the C → A transformation. In fact, the chemical rate theory of radiation-induced order-disorder transformation can be used to determine the cutoff temperature, below which amorphization can occur. In this model [56], the rate of change in the long-range order parameter consists of a disordering term due to irradiation and a thermal re-ordering term, similar to that in Sect. 9.3: dS −U = −ε K0 S + ν exp CA (1 − CA )(1 − S)2 dt kT −V S + CA (1 − CA )(1 − S)2 − exp (9.77) kT where U is the energy barrier for the A–B pair interchange, V is the ordering energy such that V = VAB − 1/2 (VAA +VBB) where VAB , VAA , and VBB are the bond energies for A–B, A–A and B–B pairs, respectively, and the remaining terms were defined in Sect. 9.3. The first term is the irradiation-induced disordering rate, and the second and third terms are the thermal re-ordering and disordering rates. An example of the variation of long-range order with temperature in the CuTi system is shown in Fig. 9.26 along with the variation of amorphization dose with temperature. Note that below about −53 ◦C, the order parameter drops to zero. This is the cut-off temperature, TC , which coincides with the onset of amorphization, Tc-a . Just above the cutoff temperature, dS/ dt is ∼ 0 and the relationship between the cutoff temperature and the damage rate, K0 , can be written by setting dS/ dt in Eq. (9.77) to zero: −U CA (1 − CA)(1 − S0)2 ε K0 S0 = ν exp kTC −V S0 − exp (9.78) S0 + CA (1 − CA )(1 − S0)2 , kT where S0 is the steady state value of the long-range order parameter. For typical values of V , the exponent inside the square brackets is of the order 10−5 to 10−21 and so the second term can be neglected, and the expression in Eq. (9.78) can be solved

474

9 Phase Stability Under Irradiation Fig. 9.26. Temperature dependence of (a) The long-range order parameter S/S0 , and (b) the critical amorphization dose for CuTi, irradiated with 1 MeV electrons (from [54])

for TC :

ν CA (1 − CA )(1 − S0)2 TC = U k ln ε K0 S0

−1 .

(9.79)

Equation (9.79) gives an estimation of the cutoff temperature, or the Tc-a temperature for a solid under irradiation. Note that it depends on the displacement rate and also on the number of replacements per displacement, ε . As such, the temperature at which amorphization will occur will depend on the irradiating particle and the dose rate. Figure 9.27 shows a schematic illustration of the temperature dependence of the critical dose for amorphization for various types of charged particles. Tc-a is the temperature below which complete amorphization can be achieved. Ta-c is the temperature beyond which the crystalline compound cannot be amorphized and is independent of irradiation conditions, and Tth is the thermal re-crystallization temperature. Okamoto et al. [54] describe the main kinetic features of irradiationinduced amorphization as follows: –

For a specified particle and dose rate, there is a temperature at which the two competing processes of damage production and recovery just balance. Below that temperature, damage production dominates recover and the crystal can be completely amorphized.

9.7 Amorphization

475

Fig. 9.27. Schematic illustration of the temperature dependence of the critical dose for amorphization for irradiation by various types of particles (from [54])

–

– – – –

Amorphization occurs homogeneously at low temperature, far from the critical dose rate and temperature. Heterogeneous amorphization occurs near the cutoff temperature. For fixed dose rate, Tc–a increases with increasing particle mass. Tc–a is a kinetic parameter that depends on the irradiation variables such as dose rate. Higher dose rates shift Tc-a to higher values. There is a temperature, Ta–c above which amorphization is impossible. Ta–c depends on the target temperature but not irradiation variables. Between Ta–c and Tth , irradiation can induce the A → C transformation and the dose required for the transformation is dose-dependent.

Figures 9.28a,b show two examples of the temperature dependence of irradiationinduced amorphization in NiAl and NiTi, respectively. Figure 9.29 shows how Tc–a varies with particle type at nearly equal dose rates. Clearly, irradiation with heavy ions can induce amorphization over a much larger temperature range than is possible by irradiation with electrons because the ions can transfer much more energy in a much smaller volume than can electrons. While electron irradiation in the ∼ MeV range produces isolated displacements (single Frenkel pairs), heavy ion irradiation results in cascades in which the effective displacement rate is high such that the damage rate outweighs the recovery rate. Relating the ordering process to the mean square static displacement, Okamoto et al. [54, 57] show that: + 2 , δstat α (1 − S2) , (9.80)

476

9 Phase Stability Under Irradiation

Fig. 9.28. Temperature dependence of the total displacement dose for ion-induced amorphization and crystallization of (a) crystalline and amorphous NiAl, and (b) crystalline and amorphous NiTi (from [54])

+ 2 , is proportional to the shear modulus, μ , then and since from Eq. (9.75), δstat μα (1 − S2 ). Figure 9.30 shows that amorphization of Zr3 Al occurs very near to the point where the straight line fit through data crosses the horizontal line for the amorphous alloy, showing that the onset of amorphization is related to a critical

9.7 Amorphization

477

Fig. 9.29. Temperature dependence of the critical amorphization dose for CuTi during irradiation with 1 MeV electrons and 1 MeV Ne, Kr and Xe ions, all at a dose rate of 10−3 dpa/s (from [54])

Fig. 9.30. Relative change in the shear modulus with increasing degree of disorder (1 − S2 ) in 1 MeV Kr+ irradiated Zr3 Al. The dashed line represents the relative shear modulus in the amorphous phase, and the vertical arrow indicates the onset of amorphization (from [54])

478

9 Phase Stability Under Irradiation

Fig. 9.31. Damage-dose dependence of the long-range order parameter, S in Zr3 Al during irradiation with 1 MeV electrons at 10 K and 320 K and with 1 MeV Kr at 295 K (from [54])

value of the mean-square chemical disorder (1 − S2) and from Eq. (9.80), the mean square static displacement. Another example of the role of disorder in amorphization is shown in Fig. 9.31 which gives the dose dependence of S for Zr3 Al during irradiation with 1 MeV electrons at two temperatures, and ions at 22 ◦C. The onset of amorphization is shown by the arrows, and although it occurs at different doses for the different particles and irradiation temperatures, the value of the order parameter is about the same. The significance of this observation is that while disordering kinetics differ between particles and temperatures, amorphization depends only on the magnitude of S and not how it is reached. Figure 9.32 [54, 57] shows an additional example of the correlation between the onset of amorphization and the rms static displacement for case of B implantation into Nb. When the mean square static displacement reaches a critical value, amorphization occurs. Radiation-Induced Amorphization Driven by Free Energy Amorphization can also be explained by considering the free energy of the transformation, as explained by Motta et al. [58, 59] and summarized here. The criteria for amorphization is that the free energy change upon irradiation, ΔGirr must be greater than that for the C → A transformation, ΔGac : ΔGirr ≥ ΔGac .

(9.81)

The term ΔGirr includes all of the defects created by irradiation and can be written as the sum of terms representing chemical disordering, ΔGdis and all other defects,

9.7 Amorphization

479

Fig. 9.32. Correlation between (a) average static displacement, δstat and (b) volume fraction of the amorphous phase vs. the concentration of B atoms implanted into Nb (after [32])

ΔGdef : ΔGirr = ΔGdef + ΔGdis = ∑ (C j E j − T ΔS j ) + ΔCAB NV − T ΔSdis ,

(9.82)

j

where C j is the concentration of defect j, E j is the formation energy, V is the ordering energy (defined earlier) and ΔS j and ΔSdis are the configuration entropy changes due to point defects and anti-site defects, respectively. The term ΔCAB is the change in the number of A–B pairs and is determined from the long-range order parameter,

480

9 Phase Stability Under Irradiation

Fig. 9.33. Plot of the dose to amorphization × square root of dose rate vs. 1/T . The lines are fit to the data and indicate that there are two regimes, an athermal regime at low temperature and a thermally activated regime at higher temperature (after [58])

S as: ΔCAB = N A 1 − S2 + B(1 − S) ,

(9.83)

where N is the number of lattice sites per mole and A and B are the fractions of atoms on the respective lattice sites in the ordered phase. The concentrations of defects is given by the defect balance equations given in Eq. (5.1). Equations (9.81), (9.82), and (9.83) and (5.1) can be used to determine a relationship between the dose to amorphization, the dose rate and the temperature. Motta determined this relationship for electron irradiation of Zr3 Fe to be: 1/2

Φa K0

i = B exp(−Em /2kT ) ,

(9.84)

i is the interstitial where Φa is the dose to amorphization, K0 is the dose rate, Em migration energy and B is a constant, and the results shown in Fig. 9.33 are found to be in good agreement with observations, shown in Fig. 9.34.

9.8 Phase Stability in Reactor Core Component Alloys The stability of phases in engineering alloys under irradiation is of great technological importance. Stainless steels are widely used in the cores of current

9.8 Phase Stability in Reactor Core Component Alloys

481

Fig. 9.34. Dose to amorphization for Zr3 Fe during electron and Ar+ irradiation (after [58])

and advanced reactor systems and have also been studied most comprehensively. Some 10 phases are observed to be affected by irradiation of austenitic stainless steels [60, 61, 62]. These phases can be grouped into three categories [60]: radiation-induced, radiation-modified, and radiation-enhanced. Table 9.2 gives the phases belonging to each category along with a crystallographic and morphological description of the phases. The radiation-induced phases include γ , G and Mx P phases and appear only under irradiation, but not under thermal conditions. The radiation-modified group consists of phases that occur during both irradiation and thermal aging and includes η (M6 C), Laves and M2 P (FeTiP). The radiationenhanced category consists of phases that regularly occur during thermal processing, but are either produced more rapidly or more abundantly at lower temperatures during reactor irradiation. Phases in this category include M6 C, M23 C6 and MC carbides and σ and χ intermetallic phases. Figure 9.35 provides a temperature-dose map in which the various phases listed in Table 9.2 are found to form. Note that while fluences of approximately 10 dpa are required for these phases to appear, the more important variable is temperature. In solution annealed and cold worked 316 SS, there is little evidence of significant radiation-induced precipitation below 370 ◦C. The only phase found to form in this regime is γ –Ni3 Si, and it has been observed in both light water reactor core components and following proton irradiation at 360 ◦C [63]. The γ phase has also been

-enhanced

-modified

-induced

Radiation

χ

Laves (A2 B) σ

M2 P (FeTiP) MC η (M6 C) τ (M23 C6 )

Laves (A2 B)

Cr3 P η (M6 C)

M2 P (FeTiP)

γ (Ni3 Si) G (M6 Ni16 Si7 )

Phase

Hexagonal, C14 P63 /mmc Same Cubic, B1 Fm3m Same Cubic, D84 Fm3m Same Tetragonal, D8b p4/mnm Cubic, A12 143m

Cubic, A1 Fm3m Cubic, A1 Fm3m Hexagonal, C22, P321 Tetragonal, S24 14 Cubic, E9, Fd3M

Crystal structure

– Rhombohedral Faulted lath

0.92 (c/a = 0.5) 1.08 0.47 (c/a = 0.77)

0.89

Same 0.88 (c/a = 0.52)

various

Same Various

Same Spherical Same Rhombohedral platelet

Thin lath

0.6 (c/a = 0.6)

Same 0.43 Same 1.06

Spherical Small rod

0.35 1.12

Lattice parameter (nm) Morphology

Table 9.2. Phases observed in austenitic stainless steel alloys after neutron irradiation (from [60] and [61])

various

Same Spherical Same Cube on cube or twin Same Various

0.05

Same ∼0

Same 0.7 Same 0.1

−0.05

∼0 0.1

−0.4

(1210)ppt ||(001)γ – Cube on cube or twin Various

−0.1 0.05

Volume misfit

Cube on cube Random

Orientation in γ matrix

482 9 Phase Stability Under Irradiation

9.8 Phase Stability in Reactor Core Component Alloys

483

Fig. 9.35. Dose and temperature dependence of precipitate phase formation in solution annealed 316 stainless steel irradiated in HFIR (after [61])

detected in 316 stainless steel irradiated in a fast reactor as low as 270 ◦C [60]. Between 400 and 550 ◦C, γ -Ni3 Si readily forms during fast reactor irradiations and is greatest in steels with higher Si and Ti contents. In mixed spectrum reactors in this temperature range, fine Cr-rich phases such as M23 C6 and M6 C form in 316 SS and Ti-rich MC forms in Ti-modified steels [60]. In the 500 to 600 ◦C temperature range, both radiation-induced and radiation-modified phases form, including the Gphase (M6 Ni16 Si7 ), M6 C Laves and phosphides and silicides. The G-phase volume fraction is a function of the Si, Ti and Nb content of the steel with volume fraction increasing with alloy composition. The appearance of these phases can be related to the effects of irradiation on phase stability. By far, the greatest effect of irradiation on precipitation in stainless steels is due to solute enrichment via radiation-induced segregation. Recall from Chap. 6 that irradiation of austenitic stainless steels causes the enrichment of Si and Ni at sinks and many of the phases appearing under irradiation are rich in one or both of these elements. Radiation-enhanced diffusion affects MC precipitation by enhancing its growth compared to that under thermal conditions. While it is expected that oversized phases are more stable under irradiation and undersized phases are less stable, of the phases given in Table 9.2, three have positive misfits of at least 10% and of those, only M6 C is stable under a wide range of irradiation conditions. Both MC and M23 C6 are oversized and will benefit from vacancy supersaturation, but also from the depletion of their main constituent, Cr, due to RIS. Conversely,

484

9 Phase Stability Under Irradiation

several of the phases that are undersized are induced or enhanced by irradiation: Laves, M2 P, γ . Clearly, the effect of solute segregation and other material and irradiation parameters play a large role in the phases that are stable under irradiation.

Nomenclature a A Ce Ci Cp D D˜ E j Em0 G ΔGp ΔG ΔGac ΔGirr ΔGdef ΔGdis h¯ ΔHf ΔHi-v ΔHc-a Jp k ko ks2 Kiv K0 L M n N px Q rc rp rj rnn R Rm

Lattice spacing Term relating to crystal structure dependence on ordering energy Matrix solute concentration Concentration of species i Concentration of solute in the precipitate Diffusion coefficient Interdiffusion coefficient Young’s modulus Migration energy for ordering of defect j Solute source term Free energy of formation of a precipitate Pseudo-free energy of formation of a precipitate Free energy change due to amorphization Free energy change due to irradiation Free energy change due to defects Free energy change due to chemical disordering Planck’s constant Heat of formation Enthalpy of defect formation Enthalpy for the crystalline to amorphous transition Precipitate nucleation rate Boltzmann’s constant Rate constant for the ordering reaction Sink strength Recombination rate constant Defect production rate Cell size Atomic mass Excess number of vacancies in a precipitate Atom number density Probability that a trap site is occupied by species x Activation energy for ordering Cascade radius Precipitate radius Recombination radius of specie j Nearest neighbor atom spacing Metal:metalloid size ratio Precipitate dissolution rate by ballistic mixing

Nomenclature

Rs R S Se Sj Sobserved S0 Sv Sx ΔSdis ΔS j t T TC Ta–c Tc–a Tg Tk Tm U V V0 VT Vc Vm Vi j x Xj Zα Zβ

α αj β βj δ + 2 ,1/2 δ + crit ,1/2 δ2 , + stat 2 1/2 δvib ε φ

Precipitate growth rate due to radiation-enhanced diffusion Gas constant Long-range order parameter Equilibrium value of order parameter Supersaturation of species j Observed long-range ordering parameter Steady state value of order parameter Vacancy supersaturation Solute supersaturation Configurational entropy change due to anti-site defects Configurational entropy change due to point defects Time Temperature Cut-off temperature Temperature above which crystal cannot be amorphized Temperature below which complete amorphization can be achieved Glass transition temperature Ideal glass transition temperature Melting temperature Energy barrier for ordering reaction Volume. Also, ordering parameter Activation energy when the long-range order parameter, S = 1. Energy reduction when a wrong A–B pair transforms to a correct A–B pair Cascade volume Molar volume Bond energy for species i and j Number of solute atoms in a precipitate Atom fraction of species j Number of α sites that are nearest neighbor to a β site Number of β sites that are nearest neighbor to a α site Constant in Eq. (9.22) Emission rate of species j Constant in Eq. (9.21) Capture rate of species j Fractional difference in volume of the precipitate relative to the matrix Critical value of means square displacement Amount of static disorder in the solid Root-mean-square thermal displacement Disordering efficiency Neutron flux

485

486

9 Phase Stability Under Irradiation

γ μ ν νj νc νw Θ Θ0 ρ ρp ρp0 ρ σ σD τ Ω ξ ζ

Particle-matrix interface energy. Also surface energy Shear modulus Poisson’s ratio Frequency factor for defect j Frequency factor for correct A–B pair Frequency factor for wrong A–B pair Re-solution rate of precipitate volume Debye temperature Density Precipitate number density Equilibrium precipitate number density Pseudo-equilibrium precipitate number density Parameter in Eq. (9.40) Displacement cross section Time constant Atomic volume Dissolution parameter in Eq. (9.32) Constant in Eq. (9.1)

Superscripts i v

Interstitial Vacancy

Subscripts d def dis e i irr m max p s th v x 0

Defective Defects Disordered Solubility Interstitials Irradiation Matrix Maximum Precipitate Solute Thermal Vacancies Solute atom Initial

Acronyms CSRO HFIR NHM

Compositional short-range order High Flux Isotope Reactor (Oak Ridge National Laboratory) Nelson–Hudson–Mazey

Problems

RED RIS TSRO

487

Radiation-enhanced diffusion Radiation-induced segregation Topological short-range order

Problems 9.1 A spherical precipitate grows via a random nucleation process at temperature T . The same precipitate grows under irradiation at the same temperature T . Under irradiation, the time to obtain the same volume fraction of precipitate is half that during pure thermal aging. Calculate the difference in the activation energy at this temperature between thermal and irradiated conditions for this transformation process. State key assumptions. 9.2 What phase is 304 stainless steel? Does radiation-induced segregation in 304 stainless steel tend to stabilize or destabilize this phase? Explain why. 9.3 For 316 SS under irradiation with a vacancy supersaturation, Sv = 104 and a solute supersaturation, Sx = 102 , find the interstitial to vacancy arrival rate ratio (βi /βv ) that will stabilize a precipitate phase that is oversized by 5% (δ = 0.05). Plot your results as a function of temperature from 573 to 873 K in increments of 100 K. Neglect the temperature dependence of Young’s modulus. 9.4 For a Ni–5%Al alloy undergoing shrinkage by recoil dissolution and growth by diffusion of the solute from solution: a) Determine the critical γ precipitate radius, below which growth occurs and above which shrinkage will occur. b) Compare your result to that expected when the precipitate size is governed by dissolution disordering. Use the following irradiation parameters:

φf = 1015 n/cm2 s (E ∼ 0.5 MeV) ρ = 1015 cm−3 ζ Ω = 10−4 nm ξ = 10 nm D = 10−15 cm2 /s 9.5 For the same alloy as in the last problem, plot the dependence of the maximum stable particle size on f , the fraction of atoms dissolved by a cascade for precipitates undergoing irradiation-induced re-solution. Make the plot for the range 0 < f < 1 and l = 10 nm. 9.6 Estimate the disordering rate due to irradiation for Ni–25Al (γ ) irradiated with 5 MeV Ni++ ions at a displacement rate of 10−3 dpa/s and with a disordering efficiency of 30. 9.7 A recent paper reports the discovery of a new microstructural defect aggreBH gate, termed a black hole because of its affinity for vacancies (zBH v > zi ).

488

9 Phase Stability Under Irradiation

Describe how the presence of these black holes along with the usual array of defect sinks will affect: a) Void nucleation rate b) Critical void size c) Void growth rate d) Incoherent precipitate (δ > 0) stability e) Incoherent precipitate nucleation rate. 9.8 In the nickel-rich end of the Ni–Al system, a solid solution of Al in Ni, known as the γ phase, has an fcc crystal structure. Near a composition of Ni–50Al, the β phase (bcc) is the stable structure. Given the information below, determine the window on Sv and βi /βv needed to form the NiAl (β ) phase from: a) A saturated solution of Al in Ni b) A supersaturated solution, Sx = 2.0 c) An undersaturated solution, Sx = 0.5. Irradiation temperature = 500 ◦C N = 0.35 E = 150 GPa aβ = 0.3574 nm aγ = 0.490 nm 9.9 Using the rules for amorphous phase formation, describe the relative ease of forming an amorphous phase in each single and two-phase region of the Ni–Al phase diagram. Explain your reasoning. 9.10 One of the theories of the formation of irradiation-induced amorphization requires that the vacancy and interstitial defect concentrations reach a level of 2%, at which point the affected volume will become amorphized. Determine whether this is possible in NiAl (β – bcc) by determining the migration enthalpy for interstitials at 300 K which would allow the point defect concentrations to reach this point. Assume a low sink concentration in the material and a displacement rate of 10−4 dpa/s. 9.11 Estimate the crystalline-to-amorphous temperature for NiAl3 for the following irradiation and material parameters under 5 MeV Ni++ ion irradiation: K0 = 10−3 dpa/s U = 0.1 eV S0 = 1.0

ν = 1013 s−1 ε = 30

References 1. Rehn LE (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier Science, New York, pp 17–33

References 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43.

489

Nelson RS , Hudson JA, Mazey DJ (1972) M Nucl Mater 44:318–330 Wilkes P (1979) J Nucl Mater 83:166–175 Brailsford AD (1980) J Nucl Mater 91:221–222 Wagner C (1961) Z Elektrochem 65:581–591 Lifshitz IM, Slyozov VV (1961) Phys Chem Solids 19:35–50 Frost HJ, Russell KC (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 75 Baron M, Chang H, Bleiberg ML (1977) In: Bleiberg ML, Bennett JW (eds) Radiation Effects in Breeder Reactor Structural Materials. TMS-AIME, New York, pp 395–404 Bilsby CF (1975) J Nucl Mater 55:125–133 Frost HJ, Russell KC (1982) Acta Metal 30:953–960 Frost HJ, Russell KC (1981) J Nucl Mater 103–104:1427–1432 Wollenberger H (1994) J Nucl Mater 2116:63–77 Abromeit C, Naundorf V, Wollenberger H (1988) J Nucl Mater 155–157:1174–1178 Russell KC (1984) Prog Mater Sci 28:229–434 Liou K-Y, Wilkes P (1979) J Nucl Mater 87:317–330 Nastasi M, Mayer JW, Hirvonen JK (1966) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge, p 342 Potter DI (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 213 Eridon J, Rehn L, Was G (1987) Nucl Instr Meth B 19/20:626 Brimhall JL, Kissinger HE, Charlot LA (1983) Rad Eff 77:273 Maydet SI, Russell KC (1977) J Nucl Mater 64:101–114 Russell KC (1979) J Nucl Mater 83:176–185 Mruzik MR, Russell KC (1978) J Nucl Mater 78:343–353 Cauvin R, Martin G (1981) Phys Rev B 32(7):3322–3332 Martin G, Bellon P, (1997) In: Ehrenreich H, Spaepen F (eds) Solid State Physics: Advances in Research and Applications, vol 50. Academic, New York, pp 189–332 Brimhall JL, Simonen EP (1986) Nucl Instr Meth B 16:187 Was GS, Eridon JM (1987) Nucl Instr Meth B 24/25:557 Was GS (1989) Prog Surf Sci 32(3/4):211 Luzzi DE, Meshii M (1986) Scr Metal 20:943 Johnson E, Wohlenberg T, Grant WA (1970) Phase Transitions 1:23 Grant WA (1981) Nucl Instr Meth 182/183:809 Johnson E, Littmark U, Johnson A, Christodoulides C (1982) Phil Mag A 45:803 Follstaedt DM (1985) Nucl Instr Meth B 78:11 Peiner E, Kopitzki K (1988) Nucl Instr Meth B 34:173 Tsaur BY, Lau SS, Mayer JW (1980) Appl Phys Lett 36:823 Tsaur BY, Lau SS, Hung LS, Mayer JW (1981) Nucl Instr Meth 182/813:1 Shectman D, Blech I, Gratias D, Cahn JW (1984) Phys Rev Lett 53:1951 Knapp JA, Follstaedt DM (1985) Phys Rev Lett 55(15):1591 Lilienfield DA, Nastasi M, Johnson HH, Ast AG, Mayer JW (1985) Phys Rev Lett 55(15):1587 Lilienfield DA, Mayer JW (1987) Mat Res Soc Symp 74. Materials Research Society, Pittsburgh, PA, p 339 Ossi PM (1977) Mater Sci Eng 90:55 Luzzi DE, Mori H, Fujita H, Meshii M (1984) Scr Metal 18:957 Pedraza DF (1987) Mater Sci Eng 90:69 Pedraza DF (1990) Rad Eff 112:11

490 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54.

55. 56. 57. 58. 59. 60. 61. 62. 63.

9 Phase Stability Under Irradiation Pedraza DF, Mansur LK (1986) Nucl Instr Meth B 16:203 Pedraza DF (1986) J Mater Res 1:425 Simonen EP (1986) Nucl Instr Meth B 16:198 Alonso JA, Somoza S (1983) Solid State Comm 48:765 Miedema AR (1973) J Less Comm Metals 32:117 Johnson WL, Cheng Y-T, Van Rossum M, Nicolet M-A (1985) Nucl Instr Meth B 7/8:657 Martin G (1984) Phys Rev B 30:1424 Swanson ML, Parsons JR, Hoelke CW (1971) Rad Eff 9:249 Brimhall JL, Kissinger HE, Pelton AR (1985) Rad Eff 90:241 Brimhall JL, Simonen EP, Kissinger HE (1973) J Nucl Mater 48:339 Okamoto PR, Lam NQ, Rehn LE (1999) In: Ehrenreich H, Spaepen F (eds) Solid State Physics: Advances in Research and Applications, vol 52. Academic, New York, pp 2–137 Lindemann FA (1910) Z Phys 11:609 Dienes GJ (1955) Acta Metal 3:549 Lam NQ, Okamoto PR, Li M (1997) J Nucl Mater 251:89–07 Motta AT, Howe LM, Okamoto PR (1999) J Nucl Mater 270:174–186 Motta AT (1997) J Nucl Mater 244:227–250 Mansur LK (1987) In: Freeman GR (ed) Kinetics of Nonhomogeneous Processes. Wiley, New York, pp 377–463 Maziasz PJ, McHargue CJ (1987) Int Mater Rev 32(4):190–218 Maziasz P (1993) J Nucl Mater 205:118–145 Was GS (2004) In: Proceedings of the 11th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, American Nuclear Society, La Grange Park, IL, pp 965–985

10 Unique Effects of Ion Irradiation

This chapter will focus on processes that are unique to ion bombardment of metals and alloys. Ion bombardment is important in fusion reactor systems in which the reaction products consist of energetic helium and hydrogen (deuterium or tritium) ions that impact the first wall and other components. In laboratory experiments, ion implantation, ion beam mixing and ion beam-assisted deposition are used to study ion–solid interactions and to create new phases and unique microstructures. The topic of ion beam modification of materials or ion–solid interactions in general is a broad subject, and a comprehensive treatment is beyond the scope of this text. (The reader is referred to several excellent texts and review articles on the subject, see for example, [1, 2, 3, 4, 5].) Rather, we will focus on processes that occur during ion–solid interactions and that result in unique microstructures or phases in the target, such as displacement mixing, preferential sputtering, Gibbsian adsorption, grain growth, etc., and the combination of these processes that together alter the target from its original state. Recall that ions not only create damage, but they contribute to a chemical change in the target by virtue of their presence. Processes affecting the surface structure and composition that are negligible under neutron irradiation (sputtering, recoil mixing, Gibbsian adsorption) can be very significant under ion irradiation. We will start with a brief introduction of ion irradiation techniques to set the stage for understanding the effects to be described later. The effects of ion irradiation on composition, microstructure and phase formation will then be presented. A final topic is the effects due to bombardment by gases at high doses and high temperature as will be experienced in the first wall of a fusion reactor, or at low temperature in a laboratory.

10.1 Ion Irradiation Techniques The modification of metal surfaces by ion beams can be accomplished by a variety of methods, each with its own advantages for particular situations. The principal methods include ion implantation, ion beam mixing, ion beam-assisted deposition and plasma ion implantation, and are shown schematically in Fig. 10.1a–d. Each of these techniques will be briefly described and considered for their capacity to alter the composition of the target.

492

10 Unique Effects of Ion Irradiation

Fig. 10.1. Ion beam surface modification by (a) direct ion implantation, (b) ion beam mixing, (c) ion beam-assisted deposition, and (d) plasma source ion implantation (from [3])

Ion implantation (II) is the bombardment of a target with a beam of ions in the energy range from a few hundred keV to several MeV. The beam is usually monoenergetic, contains a single charge state and is generally (but not always) mass analyzed. Due to the stochastic nature of the elastic collision process, the ions come to rest in a Gaussian distribution with the mean of the Gaussian centered about Rp , the projected range, with the FWHM ∼ 2.35ΔRp, where ΔRp is the standard deviation from the mean. Although it is a simple process, this technique has several disadvantages from the standpoint of modifying the surface composition. First, since the depth of the

10.1 Ion Irradiation Techniques

493

implanted distribution varies as E 1/2 , energies in the several hundred keV range that are achievable in the most common implanters, will result in projected ranges of less than 100 nm for most heavy ions. Energies in the MeV range are required to penetrate into the micrometer range. Second, sputtering will limit the concentration of the implanted specie to a value that is the reciprocal of the sputtering yield (see Sect. 10.2.1). Since sputtering yields of metals at these energies range from 2–5, the maximum concentration of implanted specie is 50 to 20%, respectively. The shape and location of the distribution can also be a drawback. In corrosion, where the composition of the top few monolayers is most important, the bulk of the modification occurs at considerably greater depths, leaving the surface lean in the implanted specie. When implantation induces a phase transformation, the effectiveness or efficiency of direct implantation is lesser still. Finally, it is often desirable to implant metal ions into pure metals or alloys to achieve a particular surface composition. As a practical matter, most commercial implanters can produce large currents of inert gases, but more elaborate measures are needed in order to produce metal ions at currents that are practical. Ion beam mixing provides an alternative to the shortcomings of direct ion implantation. Ion beam mixing (IBM) refers to the homogenization of bilayers or multilayers of elements deposited onto the surface of a target prior to bombardment. The idea behind IBM is to create a surface alloy by homogenizing alternate layers of the alloy constituents deposited in a thickness ratio so as to result in the desired final composition following mixing. IBM greatly relieves several of the shortcomings of ion implantation. First, the requirement of producing a metal ion beam is eliminated since noble gases can be used for mixing. Noble gases will not contribute a chemical effect in the solid and yet can be made into high current beams in most commercial implanters. Second, there is no restriction on the composition range since the final composition is controlled by the ratio of layer thicknesses. This also removes two other shortfalls of ion implantation, that of uniformity and surface deficiency of the implanted specie. Ion beam mixing results in a very uniform composition throughout the depth of penetration of the ion, including the very near-surface region that is problematical for ion implantation. Finally, if the elemental layers are made thin enough, the dose needed to achieve complete mixing can be orders of magnitude lower than that needed to produce concentrated alloys by direct implantation. If the process is carried out at low temperature, the result is often a metastable alloy in the form of either a supersaturated solid solution or an amorphous structure. The microstructure can then be controlled by subsequent annealing treatments. However, despite its many advantages, ion beam mixing still suffers from the same disadvantage of limited depth of penetration. The thickness of the surface is still governed by the projected range of the ion, which is in the 100 nm range for heavy ions of a few hundred keV. A solution to this problem lies in the technique of ion beam-assisted deposition. Ion beam-assisted/enhanced deposition (IBAD/IBED) refers to the growth of a film with the assistance of an ion beam. In this technique, a film is grown onto a substrate by physical vapor deposition concurrently with the bombardment by an

494

10 Unique Effects of Ion Irradiation

ion beam of low (∼1 keV) energy. The advantages of this method are numerous. First, there is virtually no limit to the thickness of film that can be modified since bombardment occurs during growth. Second, ion bombardment concurrent with vapor deposition provides for an atomically mixed interface, resulting in greater adherence. The composition gradient at the interface can be controlled by the deposition rate and the ion flux. Third, the enhanced mobility of the surface during growth allows for the control of grain size and morphology, texture, density, composition, and residual stress state. These properties are determined principally by controlling the atom deposition rate in conjunction with the ion flux (ion to atom arrival rate ratio), ion energy, fluence and species. Hence, pure metals, solid solution alloys, intermetallic compounds and a host of metal-based compounds can be grown by this technique. A final technique is plasma surface ion implantation (PSII). In this technique, the target is placed directly in the plasma source and is then pulse biased to a high negative potential (−40 to −100 keV). A plasma sheath forms around the target and ions are accelerated normal to the target surface across the plasma sheath. PSII has several potential advantages relative to conventional line-of-sight implantation including elimination of the need for target manipulation and beam rastering, elimination of target masking (retained dose problem), operation of the ion source hardware and controls are near ground potential, and easier scaling to large and/or heavy targets. All of these techniques involve energetic ion–solid interaction and the physical processes that constitute this interaction such as sputtering, Gibbsian adsorption, recoil implantation, displacement mixing, radiation-enhanced diffusion and radiationinduced segregation. These processes affect composition, microstructure and phase structure and form the basis for the observed changes in the physical and mechanical properties of the metal or alloy. Chapters 7, 8 and 9 described the microstructure and phase changes due to irradiation, and this chapter will focus on the composition effects and some additional effects unique to ion irradiation, such as grain growth, texture modification and surface morphology during high gas loading.

10.2 Composition Changes Under ion bombardment, a variety of processes occur, some of which are much more pronounced than in the case of neutron irradiation and some that are the same. Bombardment by heavy ions results in sputtering of atoms from the surface, inducing compositional changes in the near-surface region of the target. At temperatures between 0.3 and 0.5 Tm , Gibbsian adsorption causes changes in the composition of the first two atom layers, which can impact the sputtering process. The primary disordering mechanism is collisional or ballistic mixing which can be qualitatively classified into recoil implantation and cascade (isotropic) mixing. Recoil implantation refers to the direct displacement of a target atom by a bombarding ion. Indirect processes involving other target atoms are collectively called cascade mixing. Referring to experiments involving the implantation into a bilayer or a thin marker layer

10.2 Composition Changes

495

embedded in a monatomic solid, recoil implantation produces a shift and a broadening of a given initial profile while cascade mixing produces broadening. But in addition to collisional mixing, thermal processes may become important, leading to radiation-enhanced diffusion (Chap. 5). When the flux of defects to sinks becomes coupled to the flux of host atoms, radiation-induced segregation can occur, resulting in the accumulation or depletion of an alloy component at defect sinks (Chap. 6). The following subsections provide a development of the physical processes of sputtering, Gibbsian adsorption, recoil implantation and cascade mixing. Radiation-enhanced diffusion and radiation-induced segregation were described in earlier chapters and will be included only in combination with other processes to present a complete picture of composition changes under ion bombardment. 10.2.1 Sputtering Sputtering is a key element in determining surface composition under ion bombardment, primarily through the action of preferential sputtering. Different elements sputter with different probabilities, and the surface composition is a function of these probabilities. This section will briefly describe the process of physical sputtering, followed by a discussion of preferential sputtering as it affects surface compositional changes in alloys. Basic Model Surfaces of solids erode under ion bombardment. The erosion rate is characterized by the sputtering yield, Y , which is defined as the mean number of emitted atoms per incident particle. Y depends on the structure and composition of the target, parameters of the incident beam and the experimental geometry. For medium mass ions and keV energies, 0.5 ≤ Y < 20. In the sputtering process, atoms are ejected from the outer surface layers (Fig. 10.2). The bombarding ion transfers energy in collisions to the target atoms that recoil with enough energy to generate other recoils. Some of the backwarddirected recoils will intersect the surface with enough energy to escape the solid. It is these recoils that make up most of the sputtered yield, which is proportional to the number of displaced or recoil atoms. In the linear cascade regime, the number of recoils is proportional to the energy deposited per unit depth in nuclear energy loss [6, 7, 8, 9]. A collision cascade is linear if only a minor fraction of the target atoms within the cascade volume is set in motion. For a bulk cascade, this implies a low density of point defects generated. As applied to sputtering, it means that the sputter yield must be small compared to the number of target atoms located within the surface area affected by a bombarding particle. In practice, cascades in metals are close to linear except those generated by rather heavy ions bombarding heavy targets in the energy range from ∼10 keV to ∼1 MeV. The sputtering yield for particles incident on the surface can be expressed as: Y = Λ FD (E0 ) ,

(10.1)

496

10 Unique Effects of Ion Irradiation

Fig. 10.2. Schematic illustration of the re-direction of momentum from an incident ion to the backward direction resulting in sputtering

where Y is the number of atoms emitted per incident particle, E0 is the incident particle energy, Λ contains all the material properties such as surface binding energies and incident ion angular dependence, and FD is the density of deposited energy per unit depth at the surface and depends on the type, energy and direction of the incident ion and the target parameters Z2 , M2 and N. The derivation of Λ involves a description of the number of recoil atoms that can overcome the surface barrier and escape from the solid. Sigmund [6] has derived an expression for Λ using the Thomas–Fermi screening function:

Λ = 0.042/NU0 ,

(10.2)

where N is the atomic number density and U0 is the surface binding energy and can be estimated from the heat of sublimation. The deposited energy, FD is given as FD (E0 ) = α dE/ dx|n ,

(10.3)

where dE/ dx|n is the energy loss rate due to nuclear stopping and α is a correction factor that accounts for the angle of incidence of the beam to the surface and contributions due to large angle scattering events. The factor α increases with the angle of incidence due to increased energy deposition in the surface, and α also increases with M2 /M1 , again, due to greater energy deposition in the surface. Using the inverse square potential (see Eq. (1.159)), dE/ dx|n is evaluated to be: dE/ dx|n = NSn = N

π2 M1 Z1 Z2 ε 2 a , 2 M1 + M2

(10.4)

where N is the atom number density, Sn is the nuclear stopping power, a is the screening radius, ε is the unit charge, Z and M are atomic number and atomic mass, respectively, and the subscripts 1 and 2 refer to incident and target atoms, respectively. The nuclear stopping power calculated using a Thomas–Fermi cross

10.2 Composition Changes

497

section [10] is: Sn (E) = 4π aNZ1Z2 ε 2

M1 Sn (∈) , M1 + M2

(10.5)

where Sn (∈) is the reduced stopping power (from Eq. (1.142)), and the reduced energy, ∈ (from Eq. (1.137)) is: ∈=

a M2 E. M1 + M2 Z1 Z2 ε 2

(10.6)

For 1 keV Ar incident on Cu, a = 0.0103 nm and ∈= 0.008, and for 10 keV O incident on Cu, a = 0.0115 nm and ∈= 0.27. For ion energies between 1 and 10 keV, values of ∈ are in the range 0.01 to 0.3, or just below the plateau in dE/ dx|n . Using the energy-independent value of Sn (∈) of ∼0.39 eVcm2 (from Eq. (1.162)), gives dE/ dx|n ∼1240 eV/nm for Ar incident on C, and dE/ dx|n ∼320 eV/nm for O incident on Cu. Using the expression for Λ in Eq. (10.2), the sputtering yield in Eq. (10.1) becomes: Y = 0.528α Z1Z2

M1 Sn (∈) . U0 (M1 + M2 )

(10.7)

For Ar incident on Cu, NSn = dE/ dx|n = 1240 eV/nm, U0 ∼ 3 eV, α ∼ 0.25, Λ = 0.0165 nm/eV and N = 85 atoms/nm3, giving Y ∼ 5.1. Figure 10.3 shows the variation of the sputter yield with angle, atomic number of the ion, target atom– incident ion mass ratio and ion energy. Sputtering increases with departure from normal incidence because more of the ion energy is deposited close to the surface. The same is true for the dependence on Z of the ion for a fixed energy. Sputter yield is low at low energies because of the small amount of energy deposited in the surface. Similarly, since the elastic scattering cross section decreases with energy, the energy deposited in the surface region drops at high energies and the sputter yield falls. The result is a peak at intermediate energies where the energy deposition in the near-surface region is high. The sputtering yield can be used to determine the steady state concentration of the implanted specie [1] as follows. We assume that we are implanting an ion of element A in to a target of element B, where NA,B is the atomic concentration and SA,B is the sputtered flux of elements A and B. Then at any time, we have that: SB /SA = χ (NB /NA ) ,

(10.8)

where χ is the ratio of probabilities for sputtering a B atom off the surface to that for an A atom. The flux of incident A atoms, φA is related to the total sputtered flux by the sputtering yield:

φAY = SA + SB .

(10.9)

At steady state, the addition of A atoms by implantation equals that lost by sputtering so there is no net change in the total number of A atoms in the target and

498

10 Unique Effects of Ion Irradiation

Fig. 10.3. Dependence of sputter yield on (a) angle of incidence, β , where β is measured from the surface normal (from [8]), (b) atomic number of the incident ion (from [9]), (c) target atom–incident ion mass ratio through the factor α in Eq. (10.3) (from [8]), and (d) incident ion energy (from [7])

φA = SA . Substituting for SA into Eq. (10.9) yields SB = (Y − 1)φA . Substituting for SA and SB into Eq. (10.8) gives the steady state surface composition: NA /NB = χ (Y − 1)−1 .

(10.10)

For the case where χ = 1, Eq. (10.10) becomes: NA /(NA + NB ) = 1/Y ,

(10.11)

which indicates that the concentration of the implanted specie is determined directly by the sputter yield. Preferential Sputtering When energetic ions strike a target consisting of an alloy, not all of the elements of the target will be sputtered with the same yield. The yield of A atoms of an alloy per

10.2 Composition Changes

499

incident ion in the flux of sputtered atoms [11] is: YA =

∞ 0

σA (x)(CA (x)/Ω ) dx ,

(10.12)

where σ A (x) is the cross section for A atoms at a depth x ≥ 0 to be ejected from the surface, x = 0, into the region x < 0 per incoming ion, CA (x) is the atomic fraction of A in the alloy at depth x, and Ω is the mean atomic volume. We can also define the probability per unit depth, pA (x) that an A atom present at depth x is ejected by an incoming ion: pA (x) ≡ σA (x)/Ω .

(10.13)

The yield of A atoms then takes the form: YA =

∞ 0

CA (x)pA (x) dx .

(10.14)

The primary effects in alloy sputtering are those related to the individual sputtering events and the physical variables contributing to the sputter yield, and are all contained in the sputter probability, pA , which depends on the type and energy of the incoming ion, the type of the sputtered atom and its surface binding energy, etc. Since the values of the sputter probabilities, pi will differ for differing atomic species, preferential sputtering will occur. The secondary effects in alloy sputtering enter into Eq. (10.14) via the atomic concentration, CA , which gives the probability that a site is occupied by an A atom. As a consequence, the sputter yields of the alloying components will be affected through the factor CA (x) in Eq. (10.14). Practically, sputtered atoms come from a shallow layer (Fig. 10.1) with the contribution falling off exponentially with depth. The decay length is of the order of two atomic layers. Therefore, the integral in Eq. (10.14) can be replaced [6, 7, 12] by: YA = pACAs ,

(10.15)

where pA is the average total probability for an A atom present in the surface layer to be sputtered off per incident ion and CAs is the average atomic concentration of A in the surface layer, denoted by the superscript s. The thickness of this layer is not well-defined but should be taken as one or two atomic layers for determining CAs since the origin of sputtered ions is heavily weighted toward the first atomic layer. Differences in the sputter probabilities for component atoms in an alloy are caused by differences in the amounts of energy and momentum transferred to atoms of different masses, and surface binding energies. However, continued sputtering of a semi-infinite alloy target of uniform bulk composition must eventually lead to a steady state in which the composition of the flux of sputtered atoms leaving the surface equals the composition of the bulk alloy. Wiedersich et al. [11] have shown that bombardment of a binary alloy AB with a flux of ions φ (ions/cm2s) leads to an

500

10 Unique Effects of Ion Irradiation

atom removal rate given by: dN = φ (YA + YB ) . (10.16) dt Therefore, the rate at which the sputtered surface recedes can be calculated from the total rate of atom loss per unit area: δ˙ = dδ / dt = φ Ω dN/ dt = φ Ω (p Cs + p Cs ) , (10.17) A A

B B

where δ is the thickness of the surface layer removed by sputtering. They also showed that the net accumulation rate of species, i in a slab of solid at the surface of the sample, 0 ≤ x < x0 is: dNi (10.18) = φ Cib (α /Ω b ) − Yi , dt where Cib is the atomic concentration of component i of the bulk alloy, denoted by the superscript b, α is the volume removed per incident ion and Ω b is the average atomic volume of the bulk alloy. The net rate of accumulation of implanted ions is: dN0 = φ [1 − Y0] . (10.19) dt At steady state, the terms in the square brackets of Eqs. (10.18) and (10.19) must equal zero, giving: Y1 : Y2 : Y3 .... = C1b : C2b : C3b ...,

(10.20)

Y0 = 1 .

(10.21)

and

That is, the ratios of the alloy components in the sputtered flux are the same as those of the bulk alloy and their concentrations are just uniformly diluted by the re-emitted sputter ions. Note that the steady state flux of sputtered atoms contains no information on preferential sputtering. Information about preferential sputtering can be obtained from the steady state concentrations in the near-surface region via the approximation given in Eq. (10.15). Substituting Eq. (10.15) into Eq. (10.20) yields: p1 C1b C2s = , p2 C1s C2b

or

C1s C1b p2 = . C2s C2b p1

(10.22)

That is, after steady state is attained, the sputter probabilities are proportional to the ratio of the bulk and surface concentrations of the element in question. The sputter probability of the sputter ions can be obtained from the surface concentration: p0 ∼ =

1 . C0s

(10.23)

Lam and Wiedersich [13] have described the time evolution of preferential sputtering, PS on the near-surface composition for a binary alloy AB with psA > psB , i.e.,

10.2 Composition Changes

501

Fig. 10.4. Schematic description of the effect of preferential sputtering on the time evolution of the composition of the near-surface region of the sample and of the sputtered atom flux (from [13])

for the case where PS of A atoms occurs (see Fig. 10.4). Note that initially, the concentration of A atoms in the sputtered flux (top dashed line) is larger than in the bulk. However, as the surface composition changes (bottom dashed line) and the near-surface layer composition is altered, a steady state will be achieved after a certain bombardment time, when the composition of the sputtered atom flux becomes equal to the bulk composition, as dictated by the law of conservation of matter. That is, the surface concentration of A atoms will evolve to a steady state at which the higher sputtering probability of element A relative to element B, is offset by a lower A atom concentration. Consider a binary alloy, A:B such that CAb = CBb = 0.5. Then from Eq. (10.22) we have: CAs p = B . CBs pA

(10.24)

If the surface concentrations are measured to be CAs = 0.33 and CBs = 0.67, then we know that pA : pB = 2.0. Conversely, if we measure a steady state sputtered atom flux of A atoms to B atoms of 1.0 (YA : YB = 1.0), then all this tells us is that SA : SB = 1.0. That is, measuring the sputtered atom flux tells us nothing about the surface composition. We must make surface composition measurements directly and independently. 10.2.2 Gibbsian Adsorption Gibbsian adsorption (or thermal surface segregation) is the process by which the surface of an alloy re-adjusts itself to a composition different from that of the

502

10 Unique Effects of Ion Irradiation

bulk in order to lower the free energy of the alloy [14]. In metallic systems the change can be quite substantial, but the effect is confined to one or two atomic layers. The bulk composition is essentially unaffected because of the large bulkto-surface volume ratio. The re-adjustment occurs spontaneously at temperatures sufficiently high for diffusion to proceed at reasonable speed. Consider a surface layer of compositionCAs and CBs that differs from the bulk composition CAb and CBb . At equilibrium, the surface composition is related to the bulk composition [14] by: CAb CAs ΔHA = b exp − , (10.25) CBs kT CB where ΔHA is the heat of adsorption, defined as the enthalpy change associated with the exchange of an A atom in the bulk with a B atom at the surface. At elevated temperature, equilibrium is approached by a net flux, JA of A atoms described by: (10.26) JA Ω = (νAb→sCAb CBs ) − (νAs→bCAs CBb ) ξ , where ξ is the atomic layer thickness, νAb→s is the bulk-to-surface jump frequency and νAs→b is the surface-to-bulk jump frequency for atom A. The first term on the right is the flux of A atoms from the bulk to the surface and the second term is the flux of A atoms from the surface to the bulk. At equilibrium (JA = 0), or:

νAb→s CAs CBb = , νAs→b CAb CBs and substituting into Eq. (10.25) gives: ΔHA s→b b→s . νA = νA exp − kT

(10.27)

(10.28)

This says that the activation enthalpy for a surface segregating element (one that must have ΔHA < 0) for the jump back into the bulk is effectively increased by the heat of adsorption relative to the migration enthalpy in the bulk. The difference in concentration between the surface layer and the bulk is established and maintained by the reduced probability of thermally activated jumps of A atoms from the surface into the bulk. The enhanced surface concentration due to Gibbsian adsorption, GA will result in an increased loss of the segregated elements due to sputtering. Continued preferential loss of an element by GA requires that diffusion be high (T ≥ 0.5Tm ), but because sputtering enhances thermal diffusion, the effect of GA becomes significant at T ∼ = 0.3Tm . However, the athermal displacement mixing process will oppose GA. The effect of GA at steady state is to suppress the concentration in the alloy just below the surface layer to a value that maintains the surface layer concentration at the value dictated by preferential sputtering. Hence, under ion bombardment, the surface composition will be affected by both of these processes. Lam and Wiedersich [13] provided a schematic description of the dynamic behavior of the surface composition during ion bombardment resulting from the simultaneous effects of GA and PS. In the example shown in Fig. 10.5, Gibbsian adsorption

10.2 Composition Changes

503

Fig. 10.5. Schematic description of the simultaneous effects of GA and PS on the time evolution of the near-surface composition and of the sputtered atom flux (from [13])

results in a surface concentration of A atoms that is initially greater than the bulk level, shown by the step change in A atom concentration at the surface. This leads to enhanced preferential sputtering of A atoms since the sputtered atom flux is primarily from the first atom layer. Consequently, the concentration of A atoms in the subsurface layer will be reduced in an effort to re-establish thermodynamic equilibrium. After a time, t1 , the A atom concentration profile resembles the original in that there is a step-wise enrichment of A at the surface, but the surface concentration is reduced relative to the original and the concentration behind the step is reduced as well. With increasing bombardment time, the surface concentration of A continues to drop and the zone depleted in atom A increases in depth and width. Steady state is reached when the composition of the sputtered atom flux is equal to the bulk composition of the alloy. 10.2.3 Recoil Implantation The incoming ion beam imparts its momentum to the atoms (and electrons) of the solid. Hence, the momentum distribution of atoms during the displacement process is not isotropic and atoms will be re-located preferentially in the beam direction. This does not lead to any significant net atom transport in the beam direction because the solid will relax to approximately its normal density, i.e., the flux of recoiling atoms in the beam direction is compensated by a uniform flux of atoms due to relaxation in the opposite direction. In alloys, the relocation cross section and the range of the recoiling atoms depend on the charge and mass of the nucleus in such a way that generally the lighter component atoms will be transported relative to the

504

10 Unique Effects of Ion Irradiation

heavier components in the beam direction. This can be described as a flux of atoms of some of the alloy components toward deeper regions in the target, compensated by an opposite flux of the remainder of components to maintain atomic density at the proper value, i.e., the net flux of atoms is approximately zero across any plane parallel to the surface inside the target. The expression “recoil implantation” is used to describe the net transport parallel to the beam direction of some types of atoms relative to other types. The mechanics of recoil implantation have been developed by Sigmund et al. [15, 16, 17] and are summarized here. Consider the average implantation effect of a single ion (M0 , Z0 ) slowing down along a straight line to a well-defined range, R in a homogeneous binary alloy of components 1 and 2 , characterized by Mi ,Zi , and Ci with i = 1, 2, and C1 + C2 = 1. The number of i recoils created with energy (T , dT ) in element (x, dx) along its path is: NCi dxσ0i (E(x) , T ) ,

(10.29)

where E(x) is the ion energy at depth x and σ0i is the elastic scattering cross section between ions and i atoms. From LSS theory, the projected range of a recoil, Rp is:

T Rp = Ri (T ) γ0i E(x)

1/2 ,

(10.30)

where Ri is the path length and recoils are assumed to slow down on a straight line to a well-defined range, and γi j = 4Mi M j /(Mi + M j )2 . Then the total effect, Pi of the knock-on implantation is the integral of the number of recoils and their range: 1/2 R γ0i E(x) T dx σ0i (E(x), T )Ri (T ) dT . (10.31) Pi = NCi γ0i E(x) 0 0 Equation (10.31) is evaluated on the basis of power law scattering:

σi j (E, T ) = Ci j E −m T −1−m , i, j = 0, 1, 2, m 2(1−m) Mi Ci j = B1 ai j (Zi Z j )2m Mj

2/3 2/3 −1/2 ai j = B2 Zi Z j ,

0<m 0

C → 1 as t → 0

for x = 0

∞ −∞

C(x,t) dx = α , where α is the total amount of solute in the target. Assuming

that the layer is infinitely thin, the solution to Fick’s second law is: 2 −x α exp C(x,t) = √ , (10.46) 4Dt 4π Dt √ where the variance, σ 2 = 4Dt, the standard deviation, σ = 4Dt, and the full width at half maximum, FWHM = 2.35σ . From Eq. (10.44), the increment of FWHM due to cascade mixing is then:

√ 2 dE/ dx|n φ t 1/2 ∗ ∼ . ΔFWHM = 2.35 4D t = R Ed N

(10.47)

Note that the broadening of the thin film as described by ΔFWHM is proportional to (φ t)1/2 , or the effective ion mixing coefficient, 4Dt is proportional to φ t. Figure 10.8 shows that as predicted by Eq. (10.47), mixing given by 4Dt is proportional to the dose. Taking the example of 150 keV Kr+ bombardment of a Ni sample containing a thin film as in Fig. 10.7a, the dose needed to produce a ΔFWHM of 10 nm is: ΔFWHM = 10 nm ∼ =R

2 dE/ dx|n φ t Ed N

1/2 .

(10.48)

For dE/ dx|n = N σs T , then Eq. (10.48) becomes: 1/2

2σs T φ t . ΔFWHM = 10 nm ∼ =R Ed

(10.49)

For σs ∼ 1016 cm2 , T ∼ Ei = 150 keV, Ed ∼ 15 eV and R ∼ 1.5 nm, and the dose to cause a ΔFWHM of 10 nm is 8.5 ×1014 i/cm2 . If He+ is used instead of Kr+ , then the required dose is 3.5 ×1015 i/cm2 . Case 2: Pair of semi-infinite solids (bilayer) For a bilayer as shown in Fig. 10.7b, the boundary conditions are: C=0 C =C

for x < 0

at t = 0 ,

for x > 0

at t = 0 .

10.2 Composition Changes

509

Fig. 10.7. Schematic illustration of the effect of ion beam mixing on (a) a thin film, (b) a pair of semi-infinite solids (bilayer), and (c) a thin film of finite thickness (multilayer)

The solution to Fick’s second law subject to the boundary conditions is:

x C C(x,t) = . (10.50) 1 + erf √ 2 4Dt Figure 10.9 shows that as predicted by Eq. (10.50), mixing across a bilayer interface as described by 4Dt is, indeed, linear with dose for several bilayers systems, although the proportionality constant is system-dependent, as will be discussed later.

510

10 Unique Effects of Ion Irradiation

Fig. 10.8. Marker mixing data for several different markers in amorphous Si showing the relationship between the effective ion mixing diffusion coefficient, 4Dt, and the dose, φ t (from [1])

Case 3: Thin film of finite thickness (multilayer) For a layer of finite thickness, as shown in Fig. 10.7c, the boundary conditions are: C = C

for 0 < x < a

C=0

for x < 0 , x > a

and t = 0 , and t = 0 .

The solution is:

C x x−a C(x,t) = erf √ − erf √ . 2 4Dt 4Dt

(10.51)

Chemical Effects on Ion Beam Mixing Observations of mixing in binary systems reveals large differences in the amount of mixing that cannot be explained by ballistic effects. For example, mixing in the Cu– Au system is an order of magnitude higher than that in the Cu–W system [21, 22] and mixing of marker layers in Si and Ge varies significantly for elements of similar

10.2 Composition Changes

511

Fig. 10.9. Mixing of the interface vs. dose for several bilayer samples irradiated with 600 keV Xe++ ions at 77 K (from [20])

mass [23]. These systems are collisionally similar systems in that the ratio of the masses of the constituents is similar and so in a ballistic mixing model, they should behave similarly. Quite to the contrary, Fig. 10.9 showed that collisionally similar binary systems exhibited very different mixing rates. Further, mixing was occurring at 77 K where radiation-enhanced diffusion is suppressed. Johnson [24, 25, 26, 27, 28, 29] accounted for the chemical nature of the binary alloy components by first realizing that fundamentally, diffusion is driven by a chemical potential gradient, ∇μ (x) and only for ideal solutions does Fick’s law apply. More generally, for interdiffusion of two metals which form non-ideal solutions, one must relate ∇μ (x) to ∇C(x). This can be accomplished by replacing D by a modified D that accounts for the Kirkendall effect and describes diffusional

512

10 Unique Effects of Ion Irradiation

intermixing:

D =

D0ACB + D0BCA

2ΔHmix = D 1− kT

∂ ln γ (CA ) 1+ ∂ lnCA .

(10.52)

where D is the rate coefficient of unbiased mixing, γ is the activity coefficient and ΔHmix is the enthalpy of mixing given by: ΔHmix = 2δ CACB ,

δ = z[HAB − (HAA + HBB )/2] ,

(10.53)

where z is the coordination number (number of nearest neighbors) and Hi j is the potential between atom pairs, or pair enthalpies. Equation (10.52) simply says that random walk will be biased when the potential energy depends on the configuration. So mixing rates depend not only on the number of random walk steps per unit time, but also on the degree of Darken biasing. Figure 10.10 highlights the effect of ΔHmix on mixing rates for several bilayer systems. Equation Eq. (10.52) can be used to obtain a value of kTeff , the effective temperature at which diffusion occurs. [28] In the Pt–Au system, the value for kTeff is 1 – 2 eV. This means that the dominant contribution to ion mixing occurs when particle kinetic energies are of the order 1 eV! If mixing depends on the thermodynamic properties of the solid, then it should depend on the cohesive energy, ΔHcoh , which is a measure of how tightly bound

Fig. 10.10. Effect of the heat of mixing on the observed mixing rates for several binary metal systems following irradiation with 600 keV Xe++ ions at 77 K (from [24])

10.2 Composition Changes

513

Fig. 10.11. Effect of the average cohesive energy on ion mixing in several binary metal systems following irradiation with 600 keV Xe++ at 77 K (from [29])

atoms are in a solid. Indeed, if we plot d(4Dt)/ dφ vs. ΔHcoh , we note a strong correlation (Fig. 10.11). The energy range of interest, ∼1 eV correlates with the thermalized regime of a displacement cascade, which can be depicted as a thermal spike. The effect of thermal spikes on diffusion was treated by Rossi and Nastasi [30] starting with Vineyard’s thermal spike model [31] in which the non-linear Fourier equation for heat conduction in an isotropic and uniform medium is given as: ∇κ · ∇T = c

∂T , ∂t

(10.54)

where κ = κ0 T n−1 is the thermal diffusivity, c = c0 T n−1 is the specific heat capacity, κ0 and c0 are constants and n ≥ 1. At time t = 0, a cylindrical spike is introduced along an infinite straight line at constant energy density, ε , where the distance perpendicular to the axis of the cylinder is r. The initial condition for the temperature distribution is given by: Q=

c dT = (c0 /n)T n (r, 0) .

(10.55)

For zero initial ambient temperature, solution of Eq. (10.54) subject to boundary condition in Eq. (10.55), gives the temperature distribution in space and time:

T (r,t) =

nε 4πκ0t

1/n

exp(−c0 r2 /4πκ0t) .

(10.56)

514

10 Unique Effects of Ion Irradiation

Defining η as the total number of atom jumps in one spike per unit length of the spike, then analogous to thermal diffusion, we assume Arrhenius behavior for the jump rate, R such that R = A exp(−Q/kT ), then η is:

η=

2π r dr

A exp(−Q/T (r,t)) dt .

(10.57)

Integration of Eq. (10.56) yields:

η=

n3Γ (2n)Aε 2 , 8πκ0c0 Q2n

(10.58)

where Γ (2n) is the gamma function with argument 2n. For moderate temperatures, n = 1 and Eq. (10.58) becomes:

η=

Aε 2 . 8πκ cQ2

(10.59)

Referring back to Eq. (10.52) for a binary system with |ΔHmix | > 0, the effective jump rate at temperature T can be written as: Reff = A exp(−Q/kT ) [1 − 2ΔHmix/kT ] ,

(10.60)

and Eq. (10.57) becomes;

ηc =

2π r dr

A exp(−Q/kT (r,t)) [1 − 2ΔHmix/kT (r,t)] dt ,

(10.61)

where the subscript on η denotes chemical biasing. Taking n = 1 and carrying out the integral over the size and lifetime of the spike yields:

ηc =

Aε 2 (1 − 4ΔHmix/Q) . 8πκ cQ2

(10.62)

Since the activation energy scales with the cohesive energy, we take Q = −s2 ΔHcoh , where s2 is a constant. After a dose Φ (i/cm2 ), the total number of jumps in the solid is equal to ηc Φ /ρ , where ρ is the atomic density. The mixing rate is then given by: d(4Dt) = ηc rc2 /ρ , dΦ

(10.63)

where rc is a characteristic jump distance. Assuming that rc scales with the interatomic distance as rc = s1 ρ −1/3 , we obtain: d(4Dt) K1 ε 2 = 5/3 (1 + K2 ΔHmix /ΔHcoh ) , dΦ ρ (ΔHcoh )2

(10.64)

where K1 depends on κ , c and A, and K2 = 4/s2 . Equation (10.64) is plotted in Fig. 10.12 as the mixing vs. the ratio of ΔHmix /ΔHcoh for a large number of binary

10.2 Composition Changes

515

Fig. 10.12. Correlation between mixing and the ratio of ΔHmix /ΔHcoh for several metal bilayers irradiated with 600 keV Xe++ at 77 K (from [20])

systems and shows excellent correlation, indicating that the chemical effect of on beam mixing is indeed, strong even at temperatures where RED does not occur. With increasing temperature, RED contributes to mixing as well. Figure 10.13 shows the amount of intermixed silicon in a Si–Nb bilayer sample that was irradiated with Si+ ions [32]. At high temperature, the data follow an Arrhenius-type behavior with an activation energy of 0.9 eV. As the temperature is lowered, the amount of intermixing does not continue to drop, but levels out at a value that is determined by the ballistic mixing of the elements, which is temperature-dependent. Mixing induced by temperature only (thermal mixing) is shown by the solid curve on the left with an activation energy of 2.7 eV. The effect of radiation-enhanced diffusion is then the difference between the two plots that display Arrhenius behavior. Note that the low-temperature mixing is not due to

516

10 Unique Effects of Ion Irradiation

Fig. 10.13. Logarithm of the quantity of intermixed silicon vs. reciprocal temperature for a Nb–Si bilayer sample after a fluence of 1.2 × 1017 28 Si+ /cm2 . The solid line is fit to the data points of the sum of a temperature-independent part (nearly horizontal dotted line) and a thermally activated part (high slope dotted line) with an activation energy EA ∼ 0.9 eV (from [32])

an enhancement of diffusion by radiation, but rather to ballistic mixing. The total amount of mixing can be described by an effective diffusion coefficient [25] of the form: D = Dballistic + Drad exp(−Q/kT ) ,

(10.65)

where the first term on the right hand side is due to ballistic mixing and is temperature-independent, and the second term is due to radiation-enhanced diffusion and has an Arrhenius-type temperature dependence, where Q is an apparent activation energy. The temperature at which the two terms contribute equally to diffusion can be determined from Eq. (10.65) to be: Tc =

Q . k [ln(Drad /Dballistic )]

(10.66)

Assuming that there is a scaling relationship between the apparent activation energy and the cohesive energy of the matrix, ΔHcoh , i.e., Q = SΔHcoh , where S is a constant, then we obtain: Tc =

SΔHcoh . k [ln(Drad /Dballistic )]

(10.67)

10.2 Composition Changes

517

Fig. 10.14. Correlation between the average cohesive energy and the critical temperature, Tc at which mixing by radiation-enhanced diffusion equals that due to ballistic processes (from [33])

Figure 10.14 shows the critical temperature as a function of the average cohesive energy for several bilayer systems using a scaling factor, S = 0.1 [33]. Note that the critical temperature is linear with the cohesive energy, as predicted by Eq. (10.67). That the vacancy migration energy also scales with the cohesive energy means that radiation-enhanced diffusion is due to vacancy migration. In addition to homogenization of a target, displacement mixing is a very effective tool to study phase transformations under irradiation. Phase stability under irradiation was covered in Chap. 9, but ion beam mixing provides a unique opportunity to study ion-induced phase formation. Figure 10.15 shows how bilayer wedge

518

10 Unique Effects of Ion Irradiation

Fig. 10.15. Sample configuration, equilibrium phase diagram of Ni–Al and results of multilayered samples pre-annealed at 350 ◦C followed by irradiation with 500 keV Xe+ to a dose of 2 ×1015 cm2 (from [34])

samples can be made to cover the full range of composition in the Ni–Al binary system and how the phases develop as a function of composition. Figure 10.16 also shows that in most cases the phases formed are independent of whether the irradiation is by ion beam mixing, direct ion implantation of an inert element, or direct implantation of A into B or B into A. 10.2.5 Combination of Processes Affecting Surface Compositional Changes Accounting for the effects of all the processes described in the previous sections, Lam and Wiedersich [13] constructed a phenomenological model for bombardmentinduced composition modification by formulating a set of coupled partial differential equations describing the temporal and spatial evolution of defect and atom concentrations during ion bombardment of a binary alloy. The formulation was based on

10.2 Composition Changes

519

Fig. 10.16. Summary of microstructures in the Ni–Al system prepared by various ion beam treatments (from [35])

the set of diffusion and reaction rate equations, i.e., Fick’s second law with source and sink terms, describing the time rate of change of the alloy composition and defect concentrations,

∂ Cv = −∇ · (Ω Jv ) + K0 − R , ∂t ∂ Ci = −∇ · (Ω Ji ) + K0 − R , ∂t ∂ CA disp = −∇ · [(Ω JA ) − DA ∇CA ] , ∂t

(10.68) (10.69) (10.70)

where K0 and R are the locally and spatially dependent rates of production and disp recombination of vacancies and interstitials and DA is the diffusion coefficient caused solely by the displacement process. The time-dependent atom and defect concentration distributions can be determined by solving Eqs. (10.68) through (10.70) numerically for a semi-infinite target using appropriate starting and boundary conditions as described by Lam. [13, 36, 37, 38] This formulation covers the processes of DM, RED and RIS. Gibbsian adsorption and preferential sputtering can be accommodated in the model by treating the surface layer as a separate phase. Because of the structure of the phenomenological model, calculations can be made to determine the dependence of surface and subsurface compositional changes on material and irradiation variables as well as isolating the contributions of individual processes. However, because many of the parameters needed in the models are unknown, quantitative comparisons with experiment are difficult. Nevertheless, semi-quantitative modeling of bombardment-induced compositional redistribution in several binary alloys have been made. Wiedersich et al. [11, 34] provided a nice description of the effects of the different processes that occur during bombardment of an alloy and how those processes affect the surface composition. The calculations were performed with various combinations of preferential sputtering, displacement mixing, radiation-enhanced diffusion, Gibbsian adsorption and radiation-induced segregation included. Figure 10.17 shows the time evolution of the Cu concentration profiles and the location of the

520

10 Unique Effects of Ion Irradiation

Fig. 10.17. Time evolution of Cu concentration and the location of the surface in a Cu–40 at%Ni alloy bombarded with 5 keV Ar+ at 400 ◦C (from [11])

sample surface in Cu–40at%Ni bombarded with 5 keV Ar ions at 400 ◦C. Gibbsian adsorption causes an initial enrichment in the surface concentration of Cu (1 s). After 102 s, sputtering has preferentially removed Cu from the surface, resulting in a depletion of surface Cu relative to the bulk. After 4 ×103 s, steady state is achieved

10.2 Composition Changes

521

and the Cu concentration is depleted at the surface, but the depth profile continues to reflect the effect of GA. Note also the recession of the surface with increasing dose due to sputtering. Figure 10.18 shows the time dependence of the Cu concentration at the alloy surface. Note that in the absence of irradiation (curve 1), GA leads to a strong Cu enrichment in the first atom layer. Accounting only for PS and RED during irras to the steady state value, defined diation (2) causes a monotonic decrease in CCu by the sputtering probability ratio and the bulk composition. If GA is included (3), s increases rapidly at short times owing to radiation-enhanced adsorption, and CCu then decreases slowly to the steady state value. The inclusion of DM reduces the s decreases rapidly to effect of GA (4). Considering only PS, RED and RIS (5), CCu the steady state value due to the dominant effect of segregation. If GA is added (6) then the effect of RIS is masked. Finally, with the addition of DM (7), or when all s increases initially and then decreases toward the steady processes are included, CCu state value. The effect of different combinations of processes on the steady state Cu concentration profile is illustrated in Fig. 10.19.

Fig. 10.18. Effects of various combinations of Gibbsian adsorption (GA), preferential sputtering (PS), radiation-enhanced diffusion (RED), displacement mixing (DM), and radiationinduced segregation (RIS) on the time evolution of the surface concentration of Cu in Cu–40 at%Ni described in Fig. 10.17 (from [11])

522

10 Unique Effects of Ion Irradiation

Fig. 10.19. Effects of various combinations of the same five processes described in Fig. 10.18 on the steady state Cu concentration profiles (from [11])

10.2.6 Implant Re-Distribution During Ion Implantation The implantation example given in Fig. 10.17 to Fig. 10.19 was for bombardment of an alloy with an inert gas ion that plays no role as a chemical constituent of the alloy. In ion implantation, the concentration of the implanted ion is important to track, in addition to the effects of the various surfaces processes. A kinetic model was developed recently by Lam and Leaf [39] to describe the effects of these kinetic processes on the spatial re-distribution of implanted atoms during the implantation process. The effects of spatially non-uniform rates of damage and ion deposition, as well as the movement of the bombarded surface as a result of sputtering and introduction of foreign atoms into the system, were taken into account. The evolution of the implant concentration profile in time and space was calculated for various temperatures, ion energies, and ion–target combinations for a metal substrate B into which A atoms are implanted at a flux φ . The local concentrations of vacancies, B interstitial, A interstitials, A–vacancy complexes and free substitutional (A) solutes change with implantation time according to a system of kinetic equations [39] similar to those of Eqs. (10.68) through (10.70). Concurrently with the buildup of solute concentration in the host matrix, the surface is subjected to displacements both from sputtering and the introduction of foreign atoms into the system. Sputtering causes a recession of the surface while implantation causes an expansion. The net surface displacement rate is controlled by the competition between the rates of ion collection and sputtering.

10.2 Composition Changes

523

Fig. 10.20. Development of Al concentration profiles during 50 keV implantation at 500 ◦C. The normalized damage rate, K0 and ion deposition rate P are shown in the top plot and the surface displacements resulting from sputtering are indicated. Note that the concentration profiles are multiplied by factors shown in each plot (from [13])

The temporal and spatial evolution of the surface and subsurface alloy composition is obtained by solving this set of equations for a semi-infinite medium, starting from the thermodynamic equilibrium conditions. Sample calculations were performed for low and high-energy Al+ and Si+ implantations into Ni, since it is known from earlier studies that in irradiated Ni, Si segregates in the same direction as the defect fluxes whereas Al opposes the defect fluxes [40]. Re-distributions of Al and Si solutes in Ni during 50 keV implantation at 500 ◦C are shown in Fig. 10.20 and Fig. 10.21, respectively. s increases with time to a steady state value of In the Al-implantation case, CAl ∼50 at%, which is governed by the partial sputtering yield of the implant. This value

524

10 Unique Effects of Ion Irradiation

Fig. 10.21. Time evolution of the Si concentration profile during 50 keV implantation at 500 ◦C. The normalized damage rate, K0 and ion deposition rate, P are shown in the top plot. Surface displacements resulting from sputtering are indicated (from [13])

is substantially larger than that obtained in very high-energy implantation, where s sputtering is negligible and CAl is controlled by RIS. However, the total implant concentration remaining in the sample is significantly smaller because of sputtering.

10.3 Other Effects of Ion Implantation

525

Furthermore, the shape of the steady state implant profile is dictated by PS, which controls the boundary condition at the surface, and by RED and RIS. The evolution of the Si profile is rather different from that of Al, because of the different RIS behaviors. After a short implantation time, Si enrichment occurs at the surface because of RIS, and the Si distribution peak starts moving into the sample s increases monotonically, attaining interior (Fig. 10.21). With increasing time, CSi a steady state value of ∼100 at% at t ≥ 2 ×104 s. Unlike the Al case, the Si profile shows a significant shift of the implant distribution into the beyond-range region. This predicted translation of the Si distribution peak into the sample interior was consistent with experimental measurements by Mayer et al. [41] in Si-implanted Ni at elevated temperatures.

10.3 Other Effects of Ion Implantation 10.3.1 Grain Growth Ion-induced grain growth has been observed during irradiation of pure metals and multilayers. Liu and Mayer [42] observed the growth of grains of pure nickel films upon irradiation with inert gas ions, Ar, Kr and Xe in the energy range 150 to 580 keV. In their experiments, the grain size increased with dose until saturation at about 1 ×1016 i/cm2 . They found a nearly homogeneous grain size in the irradiated samples as compared to a wide spread in the grain size of thermally annealed samples. They also observed a dependence of the saturated grain size on ion species and only a weak dependence of grain size on ion dose at high doses (Fig. 10.22). The localized damage caused by the displacement spike in the vicinity of the grain boundary is the likely driving force for grain growth. The observed grain growth is explained by the re-ordering or growth of heavily damaged grains into neighboring, undamaged grains. The reduction in energy at a localized growing grain is equivalent to the difference between the energy released from the consumed region and the energy required to expand the grain boundary. The initially rapid grain growth can be explained by a larger probability of damaging an entire grain when the grains are small. As the irradiation process continues, the large grains consume the small ones and the average grain size increases. When the average diameter of the growing grains approaches the dimension of the damaged volume, the probability of highly damaging an entire grain by a single collision cascade is reduced, as is the chance of growing certain grains at the expense of others. Therefore, the grain growth rate gradually decreases with the increase of grain size. The grain growth rate during mixing of multilayered Ni–Al films is enhanced over that due to bombardment of co-deposited Ni–Al films of the same average composition by a factor of 2.2 (Fig. 10.23). This enhancement can be understood using the concept of the heat of mixing, using Johnson’s expression for the total number of atom jumps induced in a spike per unit length of a cylindrical thermal spike, η . Assuming that this value is proportional to grain boundary mobility, the

526

10 Unique Effects of Ion Irradiation

Fig. 10.22. Average grain diameter vs. dose for (a) 240 keV Ar, 310 keV Kr and 560 keV Xe ion irradiations of polycrystalline nickel films, and (b) 150 keV, 310 keV and 580 keV Kr ion irradiations of polycrystalline nickel films (from [42])

grain size, d can be related to the initial grain size, d0 and η in Eq. (10.64) as follows: 2 (d 3 − d03 )/φ αε 2 ΔHcoh [1 + K2 (ΔHmix /ΔHcoh )] .

(10.71)

10.3 Other Effects of Ion Implantation

527

Fig. 10.23. Ion-induced grain growth observed in 40 nm thick nickel, Ni–20at%Al multilayers and Ni–20at%Al co-evaporated films irradiated with 700 keV Xe++ ions (from [43])

Since ΔHmix = 0 for the irradiated co-evaporated films, the ratio of measured values of mobilities should be: (d 3 − d03 )ML / φ |ML = 1 + K2(ΔHmix /ΔHcoh ) . (10.72) (d 3 − d 3 ) / φ | 0

CO

CO

Given the cohesive energy and heat of mixing of a Ni–20at%Al alloy, the ratio in Eq. (10.72) is 3.0, as compared with the measured value of 2.2. These results indicate that the heat of mixing appears to play a role in ion-induced grain growth as well as ion beam mixing. 10.3.2 Texture There have been many reports of texture effects in ion beam mixed or ion beamassisted deposition of films. Alexander et al. [43] and Eridon et al. [44] found that mixing multilayers of Ni and Al in the composition Ni–20%Al resulted in the formation of the hcp and fcc (γ ) phases. The γ phase had a strong 111 texture and the hcp phase had a 001 texture. The textures were such that the close-packed planes of both phases were parallel to the film surface. These textures formed regardless of the angle of the ion irradiation with respect to the film. The formation of the texture seemed to be driven by the matching of the close packed planes. Ahmed and Potter [45] found that irradiation of Ni with Al to 1.2 ×1018 /cm2 resulted in 350 nm

528

10 Unique Effects of Ion Irradiation

grains of β phase oriented with respect to the underlying fcc nickel in accord with the Nishiyama relationship [46]. The development of texture during ion beam-assisted deposition can be correlated with the channeling directions of ions in the crystal lattice and the density of energy deposition would be inversely related to the depth of channeling. Thus, in an fcc crystal, the ease of channeling is in the order 110, 200, 111. Bradley et al. [47] have developed a model to explain the development of preferred orientation due to low-energy ion bombardment during film growth which is based on the difference in sputtering yields for different orientations rather than reorientation during recrystallization. Both effects are of course based on the same phenomenon of the variation of energy density with channeling direction. In this model, crystallites with high sputtering orientations are removed more rapidly and newly deposited material grows epitaxially in the low sputtering yield orientations. Thin films of PVD deposited materials normally grow with the planes of highest atomic density parallel to the substrate so fcc films have a 111 texture, bcc films have a 110 texture and hcp films have a 0002 texture (for ideal c/a ratios). The easiest channeling directions in each structure are as follows: fcc 110 , 100 , 111 bcc 111 , 100 , 110 hcp 1120 , 0002 Ion bombardment causes a shift in the preferred orientation to alignment of the easiest channeling direction along the ion beam axis. Thus, an ion beam at normal incidence on an fcc film will cause a shift in orientation from 111 to 110 texture. A beam incident at an angle will produce a different texture depending on the crystallography. The texturing effect appears to be most sensitive to high-energy beams because of the larger volume affected per ion and the deeper penetration. Experiments on ion bombardment during deposition of an Al film show that while Al forms a very strong 111 texture during physical vapor deposition, bombardment during deposition can induce an equally strong 110 texture that is driven by ion channeling [48]. 10.3.3 Dislocation Microstructure Ion implantation can induce the formation of a high dislocation density well beyond the implanted layer in response to high surface stresses caused by high doses of the implanted element [49]. Figure 10.24 shows the depth profile of the dislocation density in α -Fe resulting from implantation of various ions (C, Fe, W, Ar) at energies between 40 and 68 keV and to doses up to 1018 cm−2 . Note that while the projected ion range is less than 50 nm in all cases, the induced dislocation density peaks at between 5 and 10 μm and extends out to over 100 μm or more. The substructure is characterized by a dense dislocation network in which the dislocation density increases with dose and with the radius of the implanted ion. X-ray diffraction measurements show that the stresses exceed the yield stress and cause plastic strains in the range of 10%.

10.3 Other Effects of Ion Implantation

529

Fig. 10.24. Dislocation density vs. depth in α -Fe irradiated with 1) C: 40 keV, 1 ×1016 cm−2 , 2) C: 40 keV, 1 ×1018 cm−2 , 3) Fe: 68 keV, 1 ×1018 cm−2 , 4) W: 110 keV, 2 ×1017 cm−2 , 5) Ar: 50 keV, 2 ×1016 cm−2 , 6) Ar: 50 keV, 5 ×1016 cm−2 , 7) Ar: 50 keV, 1 ×1017 cm−2 . Irradiations 1–4 were pulsed and irradiations 5–7 were continuous (from [49])

The high density dislocation network created by ion implantation can induce recrystallization which can then affect the distribution of the implanted specie. Ahmed and Potter [45] performed a study of 180 keV Al implantation into pure Ni at 25 ◦C and at elevated temperatures (300 – 600 ◦C). At elevated temperatures, individual dislocation loops dominate the microstructure at the lowest fluences (∼1015 cm−2 ). These loops bound collections of interstitial atoms or vacancies, defects caused by the energetic Al ions penetrating the nickel structure and displacing atoms from their lattice sites. The loops climb with further implantation, intersect and react with other loops, and form complex dislocation networks after a dose of 2.1 ×1017 Al/cm2 . By a dose of 3 ×1017 Al/cm2 , three-dimensional aggregates of vacancies are present. The composition profile of Al implanted into Ni is relatively independent of temperature between 23 and 600 ◦C and for doses less than 1018 cm−2 . However, at higher doses, gross changes in the implanted distribution occur with the profile flattening and a considerable amount of Al transported to greater depths (Fig. 10.25). The same occurs following aging of room temperature implantations at 600 ◦C for 15 min. The microstructures developed at depths greater than the range of the 180 keVAl+ ions, ∼100 nm, play an important role in determining the stability of the implanted concentration profiles. Dislocation loops are present at depths near 300 nm following room temperature implantation. These loops are faulted Frank loops, 5 – 10 nm in diameter and their number density increases with fluence, reaching ∼4 ×1016 cm−2 at 3 ×1018 cm−2 .

530

10 Unique Effects of Ion Irradiation Fig. 10.25. Peak aluminum concentration plotted vs. fluence for implantation of aluminum into nickel at 500 ◦C (from [45])

However, the dislocations behind the implanted layer are removed when the material is heated to 600 ◦C. This occurs by re-crystallization, which is also responsible for the re-distribution of implanted Al. The following describes the processes occurring. Following room temperature implantation, an amorphous phase extends to a depth of ∼160 nm. Small crystal of β and γ extend from 160 nm to ∼300 nm and from ∼300 nm to ∼400 nm, respectively. Dislocations and dislocation loops extend beyond this to depths of >800 nm. Aging at 600 ◦C following room temperature implantation or implanting at high temperatures causes re-crystallization of the fine grain structure to depths of ∼ 800 nm to ∼1000 nm. In both instances, aluminum atoms must move through relatively pure nickel to accomplish the re-distribution, which is only possible if some fast diffusion process occurs. This is afforded by the small grains which form upon re-crystallization of the heavily dislocated region beyond the implanted layer and provide high angle grain boundaries for abnormally fast diffusion. The composition reaches a plateau by virtue of the limited extent of the re-crystallization. Figure 10.26 shows that the re-distribution only occurs above a threshold dose indicating the role of the radiation damage in the re-crystallization process. This example serves to tie together the roles of the implanted specie, the character of the radiation damage and the processes (re-crystallization and abnormally fast diffusion) that can be affected by implantation fields.

10.4 High Dose Gas Loading: Blistering and Exfoilation The first wall and divertor of a fusion reactor are expected to be subject to high fluxes of moderate to low-energy deuterium and helium ions created as fusion reaction products. Below 1 MeV, helium comes to rest approximately 1μm below the surface and extended exposure at high flux can lead to very high levels of

10.4 High Dose Gas Loading: Blistering and Exfoilation

531

Fig. 10.26. Aluminum concentration vs. time at 600 ◦C for fluences between 0.6 and 3.0 ×1018 i/cm2 . The phases observed in the implanted layers, symbols on curves, and those expected based on the equilibrium phase diagram (right side ordinate) are shown (from [45])

helium. At the expected temperatures (400 – 700 ◦C) and aided by the high defect concentration due to radiation damage, He will be mobile and will form bubbles as discussed in Chap. 8. The growth and coalescence of bubbles leads to the formation of blisters resulting in exfoliation of the surface as shown in Fig. 10.27. Figure 10.28a illustrates the result of high He loading a short distance beneath the surface of a metal. The bubbles are constrained to a narrow band of solid beneath the surface. There, they may grow and either coalesce to form larger bubbles or cause interbubble fracture due to the stresses between the bubbles (Fig. 10.28a). A cross sectional image of the subsurface region of a nickel sample bombarded with a high dose of He, Fig. 10.28b shows that the bubble microstructure is confined to the near-surface region. Stresses arise because the bubbles are not in equilibrium. That is, pressure due to the gas in the bubble is not balanced by the stress due to the surface tension, resulting in a radially directed stress, σrr on the bubble:

σrr = p − (2γ /r) .

(10.73)

Wolfer [52] developed an expression for the average stress field between bubbles: 2γ 4πρB 1/3 2/3 σ p = fHe − S F(S) , (10.74) μ μρΩ μΩ 3

532

10 Unique Effects of Ion Irradiation

Fig. 10.27. Surface topography of polycrystalline nickel irradiated with different doses of 100 keV He+ ions: (a) 2 × 1018 4 He/cm2 at normal incidence, (b) 2 × 1018 3 He/cm2 at normal incidence, (c) 1 × 1019 3 He/cm2 at normal incidence, (d) 2 × 1019 3 He/cm2 at 60◦ from normal, (e) 1.2 ×1020 4 He/cm2 at normal, and (f) 3.4 × 1019 3 He/cm2 at 60◦ from normal (from [50])

where μ is the shear modulus, fHe = mρB Ω , m is the number of gas atoms in a bubble, ρB is the bubble density, Ω is the atomic volume of the metal atoms, ρ is the helium density in the bubbles, γ is the surface energy and S = fHe /ρ The function

10.4 High Dose Gas Loading: Blistering and Exfoilation

533

Fig. 10.28. (a) Coalescence of bubbles below the surface of a sample loaded with a high dose of helium. (b) Cross section of a high dose, He-implanted surface layer of nickel showing the dislocations (deep), bubble lattice (middle) and connected channels (near-surface) (from [51])

F(S) is defined for a random array of bubbles and for ρ ∼ 1.0 as: F(S) = (0.827S1/3 − S)−1 .

(10.75)

534

10 Unique Effects of Ion Irradiation

Since the ultimate tensile strength determines both the ductile, transgranular fracture of fcc metals and the transgranular cleavage fracture of bcc and hcp metals, and is about 0.003 μ for fcc metals and roughly 0.01 μ for bcc metals, then σ ∼ 0.01μ . The corresponding helium concentrations needed to reach the stress to cause fracture between bubbles due to the stress are shown in Fig. 10.29, and for ρ = 1, the critical helium concentration is ∼20 − 40%. Wolfer also identifies another stress, the lateral stress, σL that is in the plane of the bubbles parallel to the surface (Fig. 10.30). The lateral stress depends on the swelling rate, S˙ according to:

σL =

˙ −SE , (1 − ν )

(10.76)

where E is the elastic modulus and ν is Poisson’s ratio. Blister formation is then a two-step process. Fracture starts at the depth, tB below the surface where σ is a maximum by growth of the bubbles to a point where the local stresses are sufficient to crack open the plane adjoining the bubbles. The penny-shaped crack then spreads until a diameter, DB is reached where the buckling condition is satisfied by the existing lateral load:

Fig. 10.29. Critical implanted He concentration vs. He concentration in the bubbles for the case of random bubbles (from [52])

10.5 Solid Phases and Inert Gas Bubble Lattices

535

Fig. 10.30. Schematic cross section of the He-implanted layer with gas bubbles and definitions of the lateral stress and the interbubble stress (from [52])

DB = 1.55 where P = −

μ , (1 − ν )P

(10.77)

σL dtB

(10.78)

tB 0

Note that experiment has identified the relationship between the blister base diameter and its thickness to be DB ∼ tBm , and this relation supports the lateral stress as the cause of blister formation [52]. Alternatively, the penny-shaped crack can continue to extend until detachment occurs, resulting in flaking and exfoliation as shown in Fig. 10.27. Very high doses of helium or implantation at high temperature often result in a sponge-type structure in which the surface consists of a series of pits as shown in Fig. 10.31. At very high temperature where bubbles are mobile, the pits may be the result of bubble intersection with the surface. However, high dose ion implantation can led to severe topological surface changes and this is the subject of much investigation.

10.5 Solid Phases and Inert Gas Bubble Lattices Implantation of noble gases to high doses at room temperature can lead to a different phenomenon: solid bubbles. Ar, Kr and Xe implanted into a variety of host metals have been observed to form solid bubbles consisting of crystals of the implanted

536

10 Unique Effects of Ion Irradiation Fig. 10.31. Holes in the surface of Nb irradiated with (a) 1.2 × 1020 He/cm2 at 23 ◦C and (b) 3 × 1017 He/cm2 at 823 ◦C (from [53])

noble gas. In Ni and Al, gases precipitate as solids with the same crystal structure as the host lattice and epitaxially aligned with the matrix. The solid phase forms at doses in the range of 1020 m−2 and the precipitate size is about 1.5 nm in Ni and up to 4.7 nm in Al [54, 55]. The lattice parameter of the precipitates is larger than that of the host and increases with the atomic mass of the inert gas. The lattice parameter increases with dose and tends toward a saturation value as shown in Fig. 10.32. Precipitate densities can be very high, in the range of 1024 m−3 . The average pressure of the solid gas can be determined from the average gas density, the lattice constant and the equation of state for the gas and is estimated to reach values in excess of 40 kbar. While the pressure required to solidify the gas at room temperature depends on the gas (8 kbar for Kr and 11.5 kbar for Ar), the calculated values are in excess of these amounts by several times. The inert gas is held in the solid state by the interatomic forces between the Kr–Kr and the Kr–Ni atoms, for the case of Kr in Ni. As the precipitate size increases, the average spacing between the gas atoms increases, decreasing the magnitude of the Kr–Kr interaction. Eventually, the decrease in gas pressure allows melting of the solid Kr. Implantation of high doses of Kr into amorphous TiCr resulted in the precipitation of crystalline Kr as in the case of crystalline

Nomenclature

537

Fig. 10.32. Lattice parameter of solid noble gas precipitates of Xe, Kr and Ar in nickel and of Kr in aluminum, as a function of fluence and implanted at room temperature (from [54] and [55])

metal hosts, but in this case, the solid Kr precipitates induced local crystallization of the host as a bcc structure. High dose implantation at room temperature can also lead to bubble lattice formation similar to the void lattices described in Chap. 8. Bubble lattices have been observed in Cu, Ni, Au, Ti and stainless steel irradiated with He or Kr. In fcc lattices, the bubbles form in densely packed rows parallel to the matrix {111} trace directions [56], and can be described by a lattice constant of order 7.6 nm, corresponding to a bubble density of ∼1025 m−3 . In hcp lattices, the bubble alignment is parallel to the basal plane, similar to that found for void ordering [57]. The formation of a bubble lattice is independent of the inert gas used and whether the gas atoms are present in bubbles in a gaseous or solid form.

Nomenclature a c dE/ dx|n d D DB D∗ D

Screening radius. Also nearest neighbor distance Specific heat capacity Ci Concentration of atom of type i Energy loss rate due to nuclear stopping Grain size Diffusion coefficient Blister diameter Effective diffusion coefficient Modified diffusion coefficient accounting for diffusional intermixing

538

E Ecoh Ed Emix F FD Hi j ΔHcoh ΔHA ΔHmix Ji k K0 m M N p pi pi P Pi Q Qi rc R

Rd Rp Rrecoil ΔRp S Si Sn SX t tB T Teff U0 Y z Z

10 Unique Effects of Ion Irradiation

Energy. Also Young’s modulus Cohesive energy Displacement energy Energy of mixing Displacement rate in dpa/s Deposited energy Potential energy between atom pairs of type i and j Cohesive energy Heat of adsorption Heat of mixing Flux of atoms of type i Boltzmann’s constant Defect production rate Number of gas atoms in a bubble Atomic mass Atom number density Gas pressure in a bubble Sputter probability of atom of type i Average total sputter probability of atom of type i Load Total effect of recoil implantation, Eq. (10.31) Activation energy Equivalent number of i atoms recoil implanted over a depth Rp Characteristic jump distance in a thermal spike Ion range. Also root mean square of an atom in a collision cascade Also vacancy–interstitial recombination rate. Also jump rate in thermal spikes Displacement rate in #/cm3 s Projected range Recoil range Standard deviation of the projected range Scaling factor Sputtered flux of atom of type i Nuclear stopping power Sputtered flux of element X Time Blister shell thickness Temperature. Also energy transferred in a collision event Effective temperature at which diffusion occurs Surface binding energy Sputter yield Coordination number Atomic number

Nomenclature

α χ δ ε ∈ φι γ Γ η κ λ Λ μ ν νis→b νib→s ρ ρB σd σs σ0,i σi σL σ Ω ξ

Constant in Eq. (10.3) Ratio of probability of sputtering a B atom to that for an A atom Thickness of surface layer removed by sputtering Unit charge. Also the energy density in the cascade Reduced energy Flux of atoms of type i Activity coefficient. Also surface energy Total jump frequency Number of atom jumps in a thermal spike per unit length of the spike Thermal diffusivity Jump length Factor in sputtering yield Eq. (10.2) containing material parameters Shear modulus. Also chemical potential Number of displacement per primary knock-on atom. Also Poisson’s ratio Surface-to-bulk jump frequency for atom i Bulk-to-surface jump frequency for atom i Atom density Gas bubble density Displacement cross section Scattering cross section Elastic scattering cross section between ions and i atoms Surface ejection cross section for atoms of type i Lateral stress in the solid Average stress Atomic volume Atomic layer thickness

Superscripts b s

Bulk Surface

Subscripts A B d P s

539

Adsorption Bubble or blister Displacement Projected Scattering

540

10 Unique Effects of Ion Irradiation

Acronyms CO DM GA FWHM IBAD IBED IBM II ML PS PSII RED RIS

Co-evaporated Displacement mixing Gibbsian adsorption Full width at half maximum Ion beam-assisted deposition Ion beam-enhanced deposition Ion beam mixing Ion implantation Multilayered Preferential sputtering Plasma source ion implantation Radiation-enhanced diffusion Radiation-induced segregation

Problems 10.1 Use the description of how a delta function distribution of particles spreads by diffusion to calculate the width of an initially sharply peaked distribution of: a) Vacancies b) Interstitials c) Self-tracer diffusing by vacancy mechanism. in Pt, after a time t = 1 min, for temperatures of 20 ◦C and 800 ◦C. 10.2 Consider a thin foil of a binary alloy in which the surface is the only defect sink. The foil is at thermal equilibrium at low temperature and is then heated instantaneously to near its melting point. Describe qualitatively the evolution of: a) The vacancy concentration b) The composition profile. 10.3 A bilayer of 50 nm Pd on top of 50 nm Ni is deposited on a silicon substrate. The layer is mixed with 300 keV Kr+ at a current of 40 μA/cm2 . Determine the sputtering yield. What is the maximum amount of Kr which can be implanted into this sample? 10.4 A Ni–1%Si alloy is heated to a temperature of 500 ◦C during irradiation by 500 keV Kr ions at a current density of 1μA/cm2 . a) What physical processes will be important in determining the surface concentration? b) If each process occurs independently of the others, what would be the effect of each on the surface composition? c) Estimate the combined effect of these processes on the surface composition and provide an argument to support your answer for the case where

Problems

541

i) Thermal processes dominate pure collisional processes ii) Pure collisional processes dominate thermal processes. Draw the composition vs. depth profile for cases (i) and (ii). B = 0.01 CSi B = 0.99 CNi

ΔHASi = −0.1 eV pSi /pNi = 2.0 ΔHmNi,v = 0.77 eV ΔHmNi,i = 0.1 eV ΔHmSi,v = 1.28 eV ΔHmSi,i = 0.15 eV RSι = 0.1176 nm RNi = 0.1245 nm CAsurface CAbulk −ΔHA = exp kT CBsurface CBbulk CAbulk CBbulk pA = surface pB CB CAsurface 10.5 A homogeneous A–B alloy of composition A–50 at%B is bombarded with 5 keV Ar ions at 400 ◦C. Given that the surface concentration following bombardment is 30% A and 70% B, describe what processes or combinations of processes could give rise to such behavior and which processes are dominant? v = migration enthalpy for A atoms by vacancies = 0.7 eV ΔHm,A v = migration enthalpy for B atoms by vacancies = 0.9 eV ΔHm,B i i ΔHm,A = ΔHm,B = migration enthalpy for A and B atoms via interstitials = 0.1 eV ΔHA = enthalpy of adsorption of A in B = −0.3 eV psA = sputtering probability for A atoms = 3 atoms/ion psB = sputtering probability for B atoms = 4 atoms/ion CA = constant × (dAv /dBv − dAi /dBi )Cv dAv α exp(−ΔHm,A /kT ) CAs /CBs = (CAb /CBb ) exp(−ΔHA /kT ) 10.6 Explain why ion beam mixing experiments often do not agree with the predictions from the ballistic theory of mixing. How would the temperature of the sample affect your answer?

542

10 Unique Effects of Ion Irradiation

10.7 A sample of polycrystalline Si is bombarded with 500 keV Al+ ions to a dose of 5 ×1015 i/cm2 . Given that Rp = 260 nm and ΔRp = 94 nm and that the damage profile has the same shape but peaks at 0.8Rp , calculate the peak damage in the material using reasonable assumptions. The distribution of ions is given by N(x) = Np exp(−X 2 ) where X = (x − Rp )/ΔRp , and Np = 0.4Ns /ΔRp. Assume that electronic stopping varies with energy as kE 1/2 where k = 1.5 × 10−16 eV1/2 cm2 . Energy transfer cross section based on inverse square law:

π 2 a2 Ea γ 1/2 8E 1/2 T 3/2 N = 3 ×1022 a/cm3 σ (E,T) =

Energy transfer cross section based on Rutherford scattering:

σ (E,T) =

π b20E γ 4T 2

Ec = 28 keV Ea = 14 keV Eb = 14 MeV Ed = 30 eV a = aB /(z1 z2 )1/6 aB = 0.053 nm b0 = z1 z2 ε 2 /η E ε 2 = 2aB ER 10.8 Explain the roles of cohesive energy and migration energy in ion beam mixing. What are the magnitudes of these energies and how can they influence ion beam mixing? Could a homogeneous alloy be unmixed? 10.9 A Cu–40%Ni target is irradiated with 100 keV Ar+ at a current density of 40 μA/cm2 . a) Determine which element will segregate to the surface under irradiation at 500 ◦C. b) On a single graph, draw the surface concentration as a function of time at 400 ◦C for the following processes: i) GA only ii) PS + RED iii) PS + RED + GA iv) PS + RED + RIS. GA = Gibbsian adsorption PS = Preferential sputtering RED = Radiation-enhanced diffusion RIS = Radiation-induced segregation Cu = 0.77 eV ΔHm,v Ni = 0.82 eV ΔHm,v Cu,Ni ΔHm,i = 0.12 eV

References

543

ΔHACu = −0.25 eV PCu = 5.5, PNi = 2.75 atoms/ion per unit concentration. 10.10 Determine the lateral load at which helium bubbles cause blistering in 316 stainless steel under the condition that the blister diameter ∼tB2 , where tB is the blister cap thickness.

References 1. Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge 2. Komarov F (1992) Ion Beam Modification of Materials. Gordon and Breach, Philadelphia 3. Was GS (1989) Prog Surf Sci 32(3/4):211–312 4. Smidt F (1990) Int Mater Rev 35(2):61–128 5. Hirvonen JK (1991) Mater Sci Rep 6:251–274 6. Sigmund P (1969) Phys Rev 184:383 7. Smith DL (1978) J Nucl Mater 75:20–31 8. Sigmund P (1981) In: Sputtering by Particle Bombardment I. Springer, Berlin Heidelberg New York, p 9 9. Winters HF (1976) In: Kaminsky M (ed) Radiation Effects in Solid Surfaces. American Chemical Society, Washington, DC, p 1 10. Lindhard J, Nielsen V, Scharff M (1968) Kgl Danske Videnskab Selskab Mat Fys Medd 36(10):1 11. Wiedersich H, Andersen HH, Lam NQ, Rehn LE, Pickering HW (1983) In: Poate JM, Foti G, Jacobson DC (eds) Surface Modification and Alloying, NATO Series on Materials Science. Plenum, New York, p 261 12. Falcone G, Sigmund P (1981) Appl Phys 25:307 13. Lam NQ, Wiedersich H (1987) Nucl Instr Meth B 18:471 14. Wynblatt P, Ku RC (1979) In: Johnson WC, Blakely JM (eds) Interfacial Segregation. American Society for Metals, Metals Park, OH, p 115 15. Sigmund P (1979) J Appl Phys 50(11):7261 16. Sigmund P, Gras-Marti A (1981) Nucl Instr Meth 182/183:25 17. Gras-Marti A, Sigmund P (1981) Nucl Instr Meth 180:211 18. Myers SM (1980) Nucl Instr Meth 168:265 19. Anderson HH (1979) Appl Phys (Germany) 18:131 20. Workman TW, Cheng YT, Johnson WL, Nicolet MA (1987) Appl Phys Lett 50(21):1485 21. Westendorp H, Wang ZL, Saris FW (1982) Nucl Instr Meth 194:453 22. Wang ZL, Westendorp JFM, Doorn S, Saris FW (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier, New York, p 59 23. Paine BM, Averback RS (1985) Nucl Instr Meth B 7/8:666 24. Johnson WL, Cheng Y-T, Van Rossum M, Nicolet M-A (1985) Nucl Instr Meth B 7/8:657 25. Van Rossum M, Cheng Y-T (1988) Defect Diffusion Forum 57/58:1 26. Cheng Y-T, Workman TW, Nicolet M-A, Johnson WL (1987) In: Beam-Solid Interactions and Transient Processes, vol 74. Materials Research Society, Pittsburgh, PA, p 419 27. Ma E, Workman TW, Johnson WL, Nicolet M-A (1989) Appl Phys Lett 54(5):413 28. Cheng Y-T, Van Rossum M, Nicolet M-A, Johnson WL (1984) Appl Phys Lett 45(2):185 29. Van Rossum M, Cheng Y-T, Nicolet M-A, Johnson WL (1985) Appl Phys Lett 46(6):610

544 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41.

42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57.

10 Unique Effects of Ion Irradiation Rossi F, Nastasi M (1991) J Appl Phys 69(3):1310 Vineyard GH (1976) Rad Eff 29:245 Matteson S, Roth J, Nicolet M, Rad Eff 42 (1979) 217–226 Cheng Y-T (1989) Phys Rev B 40(10):7403–7405 Hung LS, Mayer JW (1985) Nucl Instr Meth B 7/8:676 Was GS, Eridon JM (1987) Nucl Instr Meth B 24/25:557 Lam NQ, Leaf GK, Wiedersich H (1980) J Nucl Mater 88:289 Lam NQ, Wiedersich H (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier, New York, p 35 Lam NQ, Wiedersich H (1981) J Nucl Mater 103/104:433 Lam NQ, Leaf GK (1986) J Mater Res 1:251 Rehn LE, Okamoto PR (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 247 Mayer SGB, Milillo FF, Potter DI (1985) In: Koch CC, Liu CT, Stoloff NS (eds) HighTemperature Ordered Intermetallic Alloys, vol 39. Materials Research Society, Pittsburgh, PA, p 521 Liu JC, Mayer JW (1987) Nucl Instr Meth B 19/29:538 Alexander D, Was G, Rehn LE (1990) Materials Research Symposium, vol 157. Materials Research Society, Pittsburgh, PA, p 155 Eridon J, Rehn L, Was GS (1987) Nucl Instr Meth B 19/20:626 Ahmed M, Potter DI (1987) Acta Metal 35(9):2341 Nishiyama Z (1978) In: Fine ME, Meshii M, Wayman CM (eds) Martensitic Transformations, vol 7. Academic, New York Bradley RM, Harper JME, Smith DA (1986) J Appl Phys 60:4160 Ma Z, Was GS (1999) J Mater Res 14(10):4051–4061 Didenko AN, Kozlov EV, Sharkeev YuN, Tailashev AS, Rajabchikov AI, Pranjavichus L, Augulis L (1993) Surf Coat Technol 56:97–104 Behrisch R, Risch M, Roth J, Scherzer BMU (1976) Proceedings of the 9th Symposium on Fusion Technology. Pergamon, New York, pp 531–539 Ullmaier H (1983) Rad Eff 78:1–10 Wolfer WG (1980) J Nucl Mater 93/94:713–720 Behrisch R, Scherzer BMU (1983) Rad Eff 78:393–403 Birtcher RC, J¨ager W (1987) Ultramicroscopy 22:267–280 Liu AS, Birtcher RC (1989) Mat Res Soc Symp, vol 128. Materials Research Society, Pittsburgh, PA, pp 303–308 Johnson PR (1983) Rad Eff 78:147–156 Mazey DJ, Evans JH (1986) J Nucl Mater 138:16–18

11 Simulation of Neutron Irradiation Effects with Ions

Radiation effects research is conducted with a variety of energetic particles: neutrons, electrons, light ions and heavy ions. Energetic ions can be used to understand the effects of neutron irradiation in reactor components, and interest in this application of ion irradiation has grown in recent years for several reasons that include the avoidance of high residual radioactivity and the decline of neutron sources for materials irradiation. The damage state and microstructure resulting from ion irradiation, and thus the degree to which ion irradiation emulates neutron irradiation, depend upon the particle type and the damage rate. This chapter will begin with a brief review of the damage function, primary recoil spectrum and efficiency of defect production for various particle types. Effects of particle type on both microstructure and microchemistry will be discussed, followed by the effects of the irradiated microstructure on mechanical properties. The roles of dose, dose rate, and temperature parameters and the constraints on parameter space by each particle source will be discussed and compared against the effects of neutron irradiation.

11.1 Motivation for Using Ion Irradiation as a Surrogate for Neutron Irradiation In the 1960s and 1970s, heavy ion irradiation was developed for the purpose of simulating neutron damage in support of the fast breeder reactor program [1, 2, 3]. Ion irradiation and simultaneous He injection have also been used to simulate the effects of 14 MeV neutron damage in conjunction with the fusion reactor engineering program. The application of ion irradiation (defined here as any charged particle, including electrons) to the study of neutron irradiation damage is of interest to the light water reactor community to address issues such as stress corrosion cracking of core materials that are affected by irradiation [4, 5, 6]. Ion irradiation is also being used to understand the irradiated microstructure of reactor pressure vessel steels, Zircaloy fuel cladding, and materials for advanced reactor concepts. There is significant incentive to use ion irradiation to study neutron damage as this technique has the potential for yielding answers on basic processes in addition to the potential for enormous savings in time and money. Neutron irradiation experiments are not amenable to studies involving a wide range of conditions, which is precisely what is required for investigations of the basic damage processes. Radi-

546

11 Simulation of Neutron Irradiation Effects with Ions

ation damage simulation by ions allows easy variation of the irradiation parameters such as dose, dose rate and temperature over a wide range of values. Typical neutron irradiation experiments in test reactors require 1–3 years of incore exposure to reach appreciable fluence levels for accelerated post-irradiation testing. However, this is accompanied by at least another year of capsule design and preparation as well as disassembly and cooling. Analysis of microchemical changes by Auger electron spectroscopy (AES) or microstructural changes by energy dispersive spectroscopy via scanning transmission electron microscopy (STEM-EDS) and mechanical property or stress corrosion cracking (SCC) evaluation can take several additional years because of the precautions, special facilities and instrumentation required for handling radioactive samples. The result is that a single cycle from irradiation through microanalysis and mechanical property/SCC testing may take between three and five years. Such a long cycle length does not permit for iteration on irradiation or material conditions that is critical in any experimental research program. The long lead time required for design and irradiation also reduces flexibility in altering irradiation programs as new data becomes available. Because of the long cycle time, the requirement of special facilities and special sample handling, the costs for neutron irradiation experiments are very high. In contrast to neutron irradiation, ion (heavy, light or electrons) irradiation enjoys considerable advantages in both cycle length and cost. Ion irradiations of any type rarely require more than several tens of hours to reach damage levels in the 1–10 dpa range. Ion irradiation produces little or no residual radioactivity, allowing handling of samples without the need for special precautions. These features translate into significantly reduced cycle length and cost. The challenge is then to verify the equivalency of the results of neutron and ion irradiation. The key question that needs to be answered is how do results from neutron and charged particle irradiation experiments compare? How, for example is one to compare the results of a component irradiated in-core at 288 ◦C to a fluence of 1 ×1021 n/cm2 (E > 1 MeV) over a period of 8.5 months, with an ion irradiation experiment using 3 MeV protons at 400 ◦C to 1 dpa (displacements per atom) at a dose rate of 10−5 dpa/s (∼1 day), or 5 MeV Ni++ at 500 ◦C to 10 dpa at a dose rate of 5 ×10−3 dpa/s (∼1 hr)? The first question to resolve is the measure of radiation effect. In the irradiation assisted stress corrision cracking (IASCC) problem in LWRs, concern has centered on two effects of irradiation: segregation of major alloying elements or impurities to grain boundaries, which then cause embrittlement or enhance the intergranular stress corrosion cracking (IGSCC) process, and hardening of the matrix that results in localized deformation and embrittlement. The appropriate measure of the radiation effect in the former case would then be the alloy concentration at the grain boundary or the amount of impurity segregated to the grain boundary. This quantity is measurable by analytical techniques such as AES or STEM-EDS. For the latter case, the measure of the radiation effect would be the nature, size, density and distribution of dislocation loops, black dots and the total dislocation network, and how they impact the deformation of the alloy. Hence, spe-

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation

547

cific and measurable effects of irradiation can be determined for both neutron and ion irradiation experiments. The next concern is determining how ion irradiation translates into the environment describing neutron irradiation. That is, what are the irradiation conditions required for ion irradiation to yield the same measure of radiation effect as that for neutron irradiation? This is the key question, for in a post-irradiation test program, it is only the final state of the material that is important in the determination of equivalence, and not the path taken. Therefore, if one could devise ion irradiation experiments that yielded the same measures of irradiation effects as observed in neutron irradiation experiments, then the data obtained in post-irradiation experiments will be equivalent. In such a case, ion irradiation experiments can provide a direct substitute for neutron irradiation. While neutron irradiation will always be required to qualify materials for reactor application, ion irradiation provides a low cost and rapid means of elucidating mechanisms and screening materials for the most important variables.

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation The first problem in determining the equivalence between the measure of radiation effect in charged particle and neutron irradiation is the use of a common dose unit. Recall from the introduction that irradiated materials properties can be more successfully compared using dpa as a measure of exposure. The basic (measurable) dose unit for neutron irradiation is the fluence in (n/cm2) above some energy threshold (E > x MeV), where x is the energy threshold. For charged particles it is the integrated current or charge in units of Q/cm2 . Both of these measures can be converted to dose in units of dpa and dose rate as dpa/s using one of several models for the determination of dpa, as shown in Chap. 2. A fundamental difference between ion and neutron irradiation effects is the particle energy spectrum that arises due to the difference in how the particles are produced. Ions are produced in accelerators and emerge in monoenergetic beams with vary narrow energy widths. However, the neutron energy spectrum in a reactor extends over several orders of magnitude in energy, thus presenting a much more complicated source term for radiation damage. Figure 11.1 shows the considerable difference in neutron and ion energy spectra and also between neutron spectra in different reactors and at different locations within the reactor vessel. Another major difference in the characteristics of ions and neutrons is their depth of penetration. As shown in Fig. 2.25 of Chap. 2, ions lose energy quickly because of high electronic energy loss, giving rise to a spatially non-uniform energy deposition profile caused by the varying importance of electronic and nuclear energy loss during the slowing down process. Their penetration distances range between 0.1 and 100 μm for ion energies that can practically be achieved by laboratory-scale accelerators or implanters. By virtue of their electrical neutrality, neutrons can penetrate

548

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.1. Energy spectra of incident ions in a monoenergetic ion beam, and neutrons from a variety of reactor types (from [7])

very large distances and produce spatially flat damage profiles over many millimeters of material. As discussed in Chap. 2, the total number of displacements per atom is given by the K–P [8] or NRT [9] models. This quantity provides an adequate measure of the number of displacements created by the incoming particle irrespective of the mass of the particle. In addition to dpa, the primary recoil spectrum describes the relative number of collisions in which an energy between T and T + dT is transferred from the primary recoil atom to other target atoms. The fraction of recoils between the displacement energy Ed , and T is, from Eq. (3.11): 1 P(Ei , T ) = N

T Ed

σ (Ei , T ) dT

(11.1)

where N is the total number of primary recoils and σ (Ei , T ) is the differential cross section for a particle of energy Ei to create a recoil of energy T , and Ed is the displacement energy. The recoil fraction is shown in Fig. 3.5, which reveals only a small difference between ions of very different masses. But there is a substantial difference in the damage morphology between particles of different mass. Light ions such as electrons and protons will produce damage as isolated Frenkel pairs or in small clusters while heavy ions and neutrons produce

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation

549

damage in large clusters (see Fig. 3.7). For 1 MeV particle irradiation of copper, half the recoils for protons are produced with energies less than ∼60 eV while the same number for Kr occurs at about 150 eV. Recoils are weighted toward lower energies because of the screened Coulomb potential that controls the interactions of charged particles. For an unscreened Coulomb interaction, the probability of creating a recoil of energy T varies as 1/T 2 . However, neutrons interact as hard spheres and the probability of a creating a recoil of energy T is independent of recoil energy. In fact, a more important parameter describing the distribution of damage over the energy range is a combination of the fraction of defects of a particular energy and the damage energy. Described in Chap. 3, the weighted average recoil spectrum, W (Ei , T ) weights the primary recoil spectrum by the number of defects or the damage energy produced in each recoil: W (Ei , T ) =

ED (Ei ) =

1 ED (Ei )

Tˆ Ed

T Ed

σ (Ei , T )ED (T ) dT ,

σ (Ei , T )ED (T ) dT ,

(11.2)

(11.3)

where Tˆ is the maximum recoil energy given by Tˆ = Ei = 4Ei M1 M2 /(M1 + M2 )2 . As described in Chap. 3, for the extremes of Coulomb and hard-sphere interactions, the weighted average recoil spectra for each type of interaction is: WCoul (Ei , T ) = WHS (Ei , T ) =

ln T − ln Ed ln Tˆ − ln Ed

T 2 − Ed2 . Ed2

(11.4a)

(11.4b)

Equations (11.4a) and (11.4b) are graphed in Fig. 3.6 for 1 MeV particle irradiations of copper. The Coulomb forces extend to infinity and slowly increase as the particle approaches the target, hence the slow increase with energy. In a hard-sphere interaction, the particles and target do not feel each other until their separation reaches the hard-sphere radius at which point the repulsive force goes to infinity. A screened Coulomb potential is most appropriate for heavy ion irradiation. Note the large difference in W (Ei , T ) between the various types of irradiations. While heavy ions come closer to reproducing the energy distribution of recoils of neutrons than do light ions, neither is accurate in the tails of the distribution. This does not mean that ions are poor simulations of radiation damage, but it does mean that damage is produced differently and this difference will need to be considered when designing an irradiation program that is intended to produce microchemical and microstructural changes that match those from neutron irradiation. The actual number of defects that survive the displacement cascade and their spatial distribution in the solid will determine the effect on the irradiated microstructure. This topic was covered in Chaps. 3 and 7 by classification of defects according

550

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.2. History of point defects after creation in the displacement cascade

to their behavior in the solid. Figure 11.2 summarizes the effect of damage morphology from the viewpoint of the grain boundary and how the defect flow affects radiation-induced grain boundary segregation. Despite the equivalence in energy among the four particle types described in Fig. 3.7, the average energy transferred and the defect production efficiencies vary by almost two orders of magnitude! This is explained by the differences in the cascade morphology among the different particle types. Neutrons and heavy ions produce dense cascades that result in substantial recombination during the cooling or quenching phase. However, electrons are just capable of producing a few widely spaced Frenkel pairs that have a low probability of recombination. Protons produce small widely spaced cascades and many isolated FPs due to the Coulomb interaction and therefore, fall between the extremes in displacement efficiency defined by electrons and neutrons.

11.3 Particle Type Dependence of RIS We will focus on the comparison between four types of particle irradiation in order to outline a methodology for establishing equivalence between neutron and charged particle irradiation. We will further focus on radiation-induced segregation as the

11.3 Particle Type Dependence of RIS

551

measure of the effect of irradiation in order to compare the particles. RIS is selected because it depends only on the action of point defects, and not on their agglomeration. The irradiation parameters for the four particle types are given in Table 11.1. Each experiment is characterized by the particle type, energy and irradiation temperature, reported dose rate and reported total dose. The last column is the dose to reach a steady state RIS profile using the Perk’s model [11]. The columns labeled reported and corrected refer to RIS calculations using the nominal dose rate (reported value) and the efficiency-corrected (corrected value), respectively. The displacement efficiency is calculated using Naundorf’s model, described in Chap. 3. A quantity of interest in RIS for LWR core materials is the amount of chromium depleted from the grain boundary, or the area inside the Cr concentration profile (Fig. 11.3). In other reactor systems, other elements may be of interest due to the potential for in-reactor precipitation. The appropriate measure of depletion is somewhat questionable. One could use the grain boundary chromium value as the measure of the extent of chromium depletion. Alternatively, the FWHM of the depletion profile has been used. In fact both of these quantities are useful and can be obtained from measured depletion profiles. However, the area inside the Cr concentration profile represents changes to a volume of material and is more sensitive to changes in the profile shape than either the grain boundary value or the FWHM alone. The amount of Cr depletion is determined by integrating the concentration profile for

Fig. 11.3. Definition of the segregated area, M in a quantitative assessment of RIS

552

11 Simulation of Neutron Irradiation Effects with Ions

Table 11.1. Comparison of irradiation parameters and RIS for different particle types (from [10]) Particle type

Energy Temp Effic. (MeV) (◦C)

Electrons

1.0

450

Dose rate (dpa/s) rept’d corr’d∗

1.0

2 ×10−3 2 ×10−3

Protons

3.4

360

0.2

7×10−6

Ni ions

5.0

500

0.04

5×10−3 2×10−4

Neutrons Fission 288 reactor ∗ ∗∗

0.02

∼5 × 0−8

Total dose Dose to (dpa) steady state∗∗ (dpa) rept’d corr’d rept’d corr’d 10

10

28

28

0.2

7

3

0.4

25

7

1×10−6

1 10 1

0.02

4

9×10−10

1.4

Efficiency corrected value As calculated by the Perks model [11] for RIS

that element with distance from the grain boundary: l(t) CA0 − CA (x,t) dx , M=

(11.5)

0

where M is the segregated area, CA0 is the bulk atom concentration, CA (x,t) is the atom concentration near the surface, and l(t) is the half width of the depleted zone. Figures 11.4a,b show the amount of grain boundary chromium depletion as a function of irradiation dose (Fig. 11.4a) and time (Fig. 11.4b) for each of the four particles described in Table 11.1. The calculated values of Cr depletion for each of the particle types using reported and corrected dose rates, according to the freely migrating defect production efficiencies, are shown by the open and closed symbols, respectively. Since electrons are assumed to be 100% efficient in producing defects available to affect segregation, there is no change in the segregated area after accounting for efficiency. However, there is a difference with protons, heavy ions and neutrons, which amounts to a reduction in the amount of segregation. The difference is largest for neutrons and smallest for protons. The difference is a function of not only the displacement efficiency, but also the slope of the dose rate curves. Nevertheless, substantial differences result in the expected amounts of grain boundary segregation when the displacement efficiency is taken into account. Figure 11.5a shows the calculated amount of Cr depletion as a function of temperature for several displacement rates at steady state. Steady state is reached at different dose levels for each experiment. At a given displacement rate, the segregated area peaks at some intermediate temperature and falls off at both higher and lower temperatures. This is due to the dominance of recombination at low temperatures and back diffusion at high temperatures [10]. Also note that the effect of a decreasing displacement rate is to shift the curves to higher maxima at lower temperatures. For a given dose, a lower displacement rate yields lower steady state defect concentrations, reducing the number of defects lost to recombination, and shifting the curve to lower temperatures while increasing the degree of segregation. Figure 11.5a also shows the effect of three of the four parameters defining an experiment:

11.3 Particle Type Dependence of RIS

553

Fig. 11.4. Chromium depletion vs. (a) dose and (b) irradiation time, for several particle types, and the effect of correcting for particle efficiency (from [10])

554

11 Simulation of Neutron Irradiation Effects with Ions

particle type, temperature and dose rate. It does not show the effect of dose since this is a steady state result that is achieved at different doses for each of the experiments described in Table 11.1. Figure 11.5b shows the dose required to reach steady state as a function of temperature and dose rate. Each of the experiments is plotted for both the reported and the corrected displacement rates. Note the large difference in the dose to reach steady state between electrons and neutrons. In general, irradiation at a lower dpa rate will result in a lower dose to reach steady state and the difference is greatest for this comparison. Correspondingly, proton and heavy ion irradiation fall between neutrons and electrons for the experiments described in Table 11.1. This can be understood by considering the chemical rate equations given in Eq. (5.1), where the first term is the production rate, the second is the loss by mutual recombination and 1/2 the third is the loss by annihilation of defects at sinks. At steady state, Ci,v α K0 at low temperature and Ci,v α K0 at high temperature (see Chap. 5). So the resulting point defect concentrations are strong functions of the production rate. Figure 11.6 shows a plot of segregation as a function of temperature for particles with displacement rates characteristic of their sources. Note that the temperature at which segregation is a maximum (concentration is a minimum) shifts to higher values with increasing dose rate. This is due to the trade-off between temperature and dose rate. The temperature-dose rate interdependence for stainless steel over a wide range of temperatures and dose rates is shown in Fig. 11.7. Also noted are the regions in which reactor irradiation by neutrons, and where proton and Ni ion irradiations occur. This graph explains why the experiments conducted at the highest dose rates are also conducted at the highest temperatures. A simple method for examining the trade-off between dose rate and temperature in comparing irradiation effects from different particle types is found in the invariance requirements discussed in Chap. 8. For a given change in dose rate, we would like to know what change in temperature (at the same dose) is required to cause the same number of defects to be absorbed at sinks. The number of defects per unit volume that are lost to sinks up to time τ is: NSj =

τ

2 kSj Cj dt ,

(11.6)

0

and the ratio of ratio of vacancy loss to interstitial loss is: RS =

NSv , NSi

(11.7)

where j = v or i, and kS2 is the sink strength. The quantity NS is important in describing microstructure development involving total point defect flux to sinks (e.g., RIS). The number of defects per unit volume that have recombined up to time τ is given by: NR = Kiv

τ 0

CiCv dt ,

(11.8)

11.3 Particle Type Dependence of RIS

555

Fig. 11.5. (a) Chromium depletion, and (b) dose to reach steady state, as functions of temperature, dose rate and particle efficiency (from [10])

556

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.6. Dependence of grain boundary chromium concentration on temperature for particles with various dose rates and defect generation efficiencies (from [10])

where Kiv is the vacancy–interstitial recombination coefficient. NR is the relevant quantity for the growth of defect aggregates such as voids and loops that require partitioning of point defects to allow growth. The invariance requirements can be used to prescribe an ion irradiation temperature-dose rate combination that simulates neutron radiation. We take the example of irradiation of stainless steel under typical boiling water reactor (BWR) core irradiation conditions of ∼4.5 ×10−8 dpa/s at 288 ◦C. If we were to conduct a proton irradiation with a characteristic dose rate of 7.0 ×10−6 dpa/s, then using Eq. (8.158) with a vacancy formation energy of 1.9 eV and a vacancy migration energy of 1.3 eV, the experiment will be invariant in NS with the BWR core irradiation (e.g., RIS), for a proton irradiation at 400 ◦C. Similarly, using Eq. (8.162), an irradiation temperature of 300 ◦C will result in an invariant NR (e.g., swelling or loop growth). For a Ni++ ion irradiation at a dose rate of 10−3 dpa/s, the respective temperatures are 675 ◦C (NS invariant) and 340 ◦C (NR invariant). In other words, the temperature “shift” due to the higher dose rate is dependent on the microstructure feature of interest. Also, with increasing difference in dose rate, the ΔT between proton and ion irradiation increases substantially. The nominal irradiation temperatures selected for proton irradiation, 360 ◦C and for Ni++ irradiation, 500 ◦C represent compromises between the extremes for invariant Ns and NR .

11.4 Advantages and Disadvantages of the Various Particle Types

557

Fig. 11.7. Relation between temperature and dose rate in the context of radiation-induced segregation, and the locations of neutron, proton and nickel ion irradiations

11.4 Advantages and Disadvantages of the Various Particle Types Each particle type has its advantages and disadvantages for use in the study or emulation of radiation effects. Common disadvantages of charged particle beams are the lack of transmutation reactions and the need to use a raster-scanned beam. With the exception of some minor transmutation reactions that can occur with light ion irradiation, charged particles do not reproduce the types of transmutation reactions that occur in reactor core materials due to interaction with neutrons. The most important of these is the production of He by transmutation of Ni or B. But a second consideration is that of a raster-scanned beam in which any volume element of the target is exposed to the beam for only a fraction of the raster-scan cycle. For a typical beam scanner and beam parameters, the fraction of time that any particular volume element in the solid is being bombarded is ∼0.025. Thus, the instantaneous dose rate during the beam-on portion of the cycle is 40 times that of the average (Fig. 11.8). The result is that the defect production rate is very high and defects can anneal out in the remaining 0.975 portion of the cycle before the beam again passes through the volume element. As such, the effective defect production rate in raster-scanned systems will be less, and must be accounted for. While one objective of ion irradiation is to emulate the effect of neutrons, a second is to understand basic physical radiation damage processes, for which neutron

558

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.8. The effect of a raster-scanned beam on the instantaneous production rate of point defects with the same time averaged rate as a continuous source (from [12])

irradiation is often less well-suited. While ion irradiation can be conducted with great control over temperature, dose rate and total dose, such control is a challenge to reactor irradiations. For example, instrumented tubes with active temperature control are expensive to design, build and operate. Even so, frequent power changes can be difficult to handle as the flux-temperature relationship will change and this can result in artifacts in the irradiated microstructure (see Sect. 8.3.11 and Fig. 8.51). On the other hand, cheaper “rabbit” tube irradiations use passive gamma heating and temperatures are not known with any certainty. Similarly, doses and dose rates are most often determined by neutronic models of the core locations and are not verifiable. As such, ion irradiations enjoy the advantage of better control and verification of irradiation conditions as compared to neutron irradiation. Table 11.2 provides a list of advantages and disadvantages for each of three particle types; electrons, heavy ions and light ions (protons), and they are discussed in detail in the following sections. 11.4.1 Electrons Electron irradiation is easily conducted in a high voltage transmission electron microscope and as such, it uses a rather simple ion source, that being either a hot filament or a field emission gun. An advantage is that the same instrument used for irradiation damage can be used to image the damage. Another advantage is that the

11.4 Advantages and Disadvantages of the Various Particle Types

559

Table 11.2. Advantages and disadvantages of irradiations with various particle types (from [12]) Electrons Advantages Disadvantages Relatively “simple” source – TEM Energy limited to ∼1 MeV Uses standard TEM sample no cascades High dose rate – short irradiation times Very high beam current (high dpa rate) requires high temperature Poor control of sample temperature Strong “Gaussian” shape (nonuniform intensity profile) to beam No transmutation Heavy Ions Advantages Disadvantages High dose rate – short irradiation times Very limited depth of penetration Strongly peaked damage profile High Tavg Cascade production Very high beam current (high dpa rate) requires high temperature No transmutation Potential for composition changes at high dose via implanted ion Advantages Accelerated dose rate – moderate irradiation times Modest ΔT required Good depth of penetration Flat damage profile over tens of μ m

Protons Disadvantages Minor sample activation Smaller, widely separated cascades No transmutation

high dose rate requires very short irradiation time, but this will also require a large temperature shift as explained in the previous section. There are several disadvantages to electron irradiation using a TEM. First, energies are generally limited to 1 MeV. This energy is sufficient to produce an isolated Frenkel pair in transition metals, but not cascades. The high dose rate requires high temperatures that must be closely monitored and controlled, which is difficult to do precisely in a typical TEM sample stage. Another drawback is that since irradiations are often conducted on thin foils, defects are created in close proximity to the surface and their behavior may be affected by the presence of the surface. Perhaps the most serious drawback is the Gaussian shape to the electron beam that can give rise to strong dose rate gradients across the irradiated region. Figure 11.9 shows the composition profile of copper around a grain boundary in Ni–39%Cu following electron irradiation. Note that while there is local depletion at the grain boundary (as expecte

Gary S. Was

Fundamentals of Radiation Materials Science Metals and Alloys

With 381 Figures

123

Gary S. Was Nuclear Engineering and Radiological Sciences Materials Science and Engineering University of Michigan 1921 Cooley Bldg. 2355 Bonisteel Blvd. Ann Arbor, MI 48109-2104, USA e-mail: [email protected]

Library of Congress Control Number: 2007922926

ISBN 978-3-540-49471-3 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable for prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media springer.com c Springer-Verlag Berlin Heidelberg 2007 The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Typesetting and production: LE-TEX Jelonek, Schmidt & V¨ockler GbR, Leipzig Cover design: eStudio Calamar S.L., F. Steinen-Broo, Girona, Spain Printed on acid-free paper

54/3180/YL – 5 4 3 2 1 0

This book is dedicated to my wife, LeeAnn

Preface

The purpose of this text is to provide a foundation for understanding the theory and mechanisms behind the effects of irradiation on metals and alloys. The subject is divided into three parts, each of which is subdivided into individual chapters that together, provide a unified picture of how radiation interacts with, and alters the structure and properties of metallic materials. Part I consists of three chapters and focuses on the radiation damage process and provides the formalism for the prediction of the amount and spatial configuration of the damage produced by bombarding particles. Chapter 1 treats the interactions between particles that result in the transfer of energy from the incident particle to the target atoms. Chapter 2 focuses on determination of the number of displacements produced by the bombarding particles, and Chap. 3 describes the spatial configurations of the resulting defects. While radiation damage describes the state of the irradiated material, radiation effects are concerned with defect behavior in the solid after formation. Part II (Chaps. 4–11) covers the physical effects of irradiation on metals. Chapter 4 provides background on the equilibrium concentration of point defects and their diffusion. Chapter 5 treats diffusion and reactions between point defects under irradiation that are fundamental to all of the observable effects. Chapter 6 describes radiation-induced segregation, which is a direct consequence of radiation-enhanced diffusion. Chapters 7 and 8 address the nucleation and growth of dislocation loops and voids, the defect aggregates that determine much of the behavior of irradiated alloys. Chapter 9 covers the stability of phases under irradiation and irradiationinduced precipitation and precipitate dissolution. Chapter 10 extends the effects of irradiation to the unique effects resulting from ion irradiation such as composition changes, sputtering, exfoliation, etc. Finally, Chap. 11 describes the application of ion irradiation to simulate the effects of neutron irradiation. Mechanical effects of radiation damage (Part III) are distinguished from physical effects by the application of stress. Hardening and deformation of alloys under irradiation are discussed in Chap. 12. The effect of irradiation on crack nucleation and propagation resulting either from static or fatigue loading is discussed in Chap. 13. Finally, creep deformation and growth are treated in Chap. 14. Irradiation also has a profound effect on corrosion and stress corrosion cracking and these degradation modes may prove to be limiting processes for many reactor designs. Chapter 15 combines the effects of irradiation with the processes of corrosion and stress corrosion cracking to examine how irradiation and the media can combine to degrade alloy behavior.

VIII

Preface

The chapters contain examples and illustrations of radiation effects and sample calculations to quantify and describe the observations. Problems at the end of each chapter are designed to reinforce the main concepts of each chapter and to challenge the reader on his or her comprehension of the topics covered within. Taken together, the chapter text, examples, illustrations and end-of-chapter problems provide a comprehensive treatment of the effects of irradiation on metals and alloys. The subject matter in this text will likely require two academic terms to complete. Many of the topics rely on a basic knowledge of disciplines that constitute the underlying basis for irradiation effects: thermodynamics and kinetics of solids, crystal structure, defects and dislocations, physical metallurgy, elasticity and plasticity, deformation and fracture and corrosion and stress corrosion cracking. The text either presents the requisite background for each of these topics, or provides references of other sources where good treatments can be found. This book should also be useful to researchers who would like to learn more about the subject, or who would like a more complete and integrated treatment of the topics than can be found in individual papers on the subject. While the chapters are integrated with one another and each chapter builds upon the sum of the previous chapters, it is possible to read selected chapters for just that topic. As a final comment, the author would like to note that this book was written by sorting, organizing and condensing information from several texts and numerous journal and conference papers in order to arrive at a comprehensive description of the processes constituting radiation materials science. A conscientious effort was made to acknowledge and give credit to the original sources of the ideas, theories, mathematical developments and drawings contained herein. For occasional oversights that may have occurred during the condensation process, the author offers his apologies. He is indebted to the many authors and publishers who provided material and illustrations for this text. Finally, the author wishes to acknowledge the many colleagues, students and friends who aided and advised him in this work. In particular, special thanks go to Jeremy Busby, Todd Allen, Michael Atzmon, Roger Stoller, Yuri Osetsky, Ian Robertson and Brian Wirth, for their substantive contributions to the content, to Elaine West, Brian Wagner and Sean Lemecha for their work on the illustrations, to Cherilyn Davis and Ovidiu Toader for their help in manuscript and movie preparation, to Lynn Rehn, Don Olander, Arthur Motta, Michael Nastasi, Steve Zinkle, K. Linga Murty, Lou Mansur and Peter Andresen for their chapter reviews, and to John King and Arden Bement for providing the inspiration to the author to pursue this field many years ago.

Ann Arbor, May 2007

Gary S. Was

Introduction

Radiation materials science describes the interaction of radiation with matter— a broad subject covering many forms of irradiation and of matter. Some of the most profound effects of irradiation on materials occur in the core of nuclear power reactors where atoms comprising the structural components are displaced numerous times over the course of their engineering lifetimes. The consequences of radiation to core components includes changes in shape and volume by tens of percent, increases in hardness by factors of five or more, severe reduction in ductility and increased embrittlement, and susceptibility to environmentally induced cracking. For these structures to fulfill their purpose, a firm understanding of the effect of radiation on materials is required in order to account for irradiation effects in design, to mitigate its effect by changing operating conditions, or to serve as a guide for creating new, more radiation-tolerant materials that can better serve their purpose. The attractiveness of nuclear power as a present day and future energy source is due to the vast improvements that have been made in the way reactors are operated and in our understanding of how these engineering systems degrade and fail. But the attractiveness of nuclear power is also driven by new concepts for advanced reactors that offer improvements in safety and reliability, radioactive waste production, energy efficiency and cost effectiveness. Nuclear power holds the promise for producing hydrogen in a clean and low cost process that would power a future hydrogen economy. Yet all of these improvements come at a cost. That cost is a greater demand on the materials used to build and operate these reactors. New concepts that promise better performance from this energy source also include more aggressive environments, higher temperatures and greater levels of irradiation. In his article in Nature, Butler [1] summarizes the challenges facing several promising advanced reactor concepts. In all but one, material behavior is the leading challenge in bridging the gap from concept to reality. The pivotal role of material behavior in the unique radiation environment created in a reactor core makes radiation materials science of paramount importance in the future of nuclear energy in the world. It is with this perspective that the objective of this text was formulated, to provide a sound, fundamental understanding of radiation effects in structural materials. Structural materials in reactor systems are predominantly crystalline, metallic alloys. Virtually all of the structural materials in reactors are metallic, and many of the materials proposed for the more aggressive conditions in advanced reactor concepts are metals as well. The types of radiation that can alter structural materials

X

Introduction

consist of neutrons, ions, electrons and gamma rays. All of these forms of radiation have the capability to displace atoms from their lattice sites, which is the fundamental process that drives the changes in structural metals described earlier. The inclusion of ions among the irradiating particles provides a tie-in to other fields and disciplines such as the use of accelerators for the transmutation of nuclear waste, or in the creation of new materials by ion implantation, ion beam mixing, plasma assisted ion implantation and ion beam assisted deposition. All of the concepts developed in this text for the interactions of ions with solids are applicable to these fields as well. The effect of irradiation on materials is rooted in the initial event in which an energetic projectile strikes a target. While the event is made up of several steps or processes, the primary result is the displacement of an atom from its lattice site. This book will address primarily crystalline solids in which the atom locations are defined by the crystalline structure. Irradiation displaces an atom from its site, leaving a vacant site behind (a vacancy) and the displaced atom eventually comes to rest in a location that is between lattice sites, becoming an interstitial atom. The vacancyinterstitial pair is central to radiation effects in crystalline solids and is known as a Frenkel pair (FP). The presence of the Frenkel pair and other consequences of irradiation damage determine the physical effects, and with the application of stress, the mechanical effects of irradiation. The radiation damage event, detailed in Chap. 1, is concluded when the displaced atom (also known as the primary knock-on atom, PKA) comes to rest in the lattice as an interstitial. This event consumes about 10−11 s. Subsequent events are classified as physical effects of irradiation. These effects include such phenomena as swelling, growth, phase change, segregation, etc. For example, it is possible to take a block of pure nickel, 1 cm on a side, irradiate it in a reactor (to a fluence of say, 1022 n/cm2 ) and measure it to be 1.06 cm on a side, representing a volume change of 20%! The volume change, or swelling, is isotropic and is due to the formation of voids in the solid (see for example, Fig. 8.1). Another example is irradiation growth. One can irradiate a cylindrical rod of uranium, 10 cm in length and 1 cm in diameter (7.85 cm3 ) to a fluence of ∼1020 n/cm2 and measure it to be 30 cm in length and 0.58 cm in diameter. The volume is unchanged (7.85 cm3 ), but the shape is highly distorted. Distortion at constant volume under irradiation is referred to as growth. Phase changes under irradiation are also common. A Ni–12.8at%Al, solid solution alloy irradiated with 5 MeV Ni+ ions to 1016 cm−2 will result in the formation of a Ni3 Al phase, which is separate and distinct from the parent phase (see for example, Fig. 9.3). The formation of a new phase is known as irradiation-induced phase formation and is of great significance in both ion and neutron irradiations. A last example of physical changes of irradiation is segregation. If a Ni–1at%Si alloy is bombarded with Ni+ ions at 525 ◦C and to a dose of one displacement per atom, the result is an enrichment of Si on the surface and at grain boundaries to values that are 20 to 60 times the amount in the bulk (see for example, Fig. 6.5). This redistribution of alloying elements to specific sites in the microstructure is

Introduction

XI

known as radiation-induced segregation and occurs in many alloys to a significant extent when irradiated at high temperatures. Irradiation-induced physical changes can indeed be dramatic. But how do they alter the structural integrity of components? This is the realm of mechanical effects of irradiation. Mechanical effects manifest themselves only under the application of a stress. The result is that alloys behave much differently than their unirradiated counterparts. For example, the impact energy of an irradiated steel can be drastically reduced. For unirradiated steels, the energy absorbed is a strong function of temperature, where at low temperatures, little energy is absorbed and the steel becomes very brittle, but with increasing temperature, the energy absorbing capacity of the steel increases dramatically. Irradiation of a steel with neutrons can cause a marked reduction in the strain and a several-fold increase in the strength of the steel. The result is an increase in strength by a factor of five and a decrease in ductility by over a factor of ten. Irradiation can also influence the way in which materials deform at high temperature. Under a constant load, there is almost a complete loss of creep strength due to severe embrittlement arising from irradiation. Finally, irradiation to a neutron fluence of >5 × 1020 n/cm2 (E > 1 MeV) results in accelerated intergranular cracking of iron- and nickel-base austenitic alloys in light water reactors. This cracking phenomenon is very pervasive in that it affects most all austenitic alloys in all types of water reactors. Clearly, any of these effects will have profound consequences on reactor component integrity. Understanding how they work is the key to designing around their detrimental effects or to developing new alloys that are more radiation tolerant. As it turns out, almost all of these effects have a common link: defects such as isolated vacancies and interstitials, clusters of vacancies and interstitials, dislocation loops and lines and voids and bubbles. The reader should keep these defect types in mind as we move from the radiation damage event through the physical effects to the mechanical effects. We will address the radiation damage event first as this is the basis for understanding all effects of irradiation. We will start by quantifying the extent of radiation damage and develop a physical description of the interaction process. In quantifying the displacement process, what we are seeking is a quantitative description of the number of vacancies and interstitials produced by an incoming projectile. Unless we can do this, we have no hope of understanding the extent of the damage. The importance of determining the effect of irradiation in terms of the production of defects is discussed in Chaps. 2 and 3, and is shown here with a simple illustration. The number of displacements created by a neutron flux is a complicated function of the energy dependence of that flux. Note in the top graph in Fig. I.1 that the dependence of the yield strength of a 316 stainless steel alloy on the neutron fluence is highly dependent on the particular neutron flux spectrum [2]. OWR is a test reactor with a typical LWR neutron spectrum, RTNS-II produced a pure 14 MeV source of neutrons and LASREF had a broad spectrum of high neutron energies. However, if the yield strength is plotted as a function of the displacement damage in the alloy (dpa = displacements per atom in the solid), then data from all three neutron sources collapses beautifully onto a single trend line (bottom graph in Fig. I.1) that

XII

Introduction

Fig. I.1. Comparison of yield stress change in 316 stainless steel irradiated in three facilities with very different neutron energy flux spectra. While there is little correlation in terms of neutron fluence, the yield stress changes correlate well against displacements per atom, dpa (after [2])

References

XIII

is independent of the flux spectrum. The independence of the yield strength-dpa correlation on the neutron spectrum indicates that dpa is a better representation of the effect of irradiation on materials properties than is the fluence, giving rise to our first objective. That is the determination of the quantity R, the number of displacements per unit volume per unit time: #displacements =N R≡ cm3 s

Eˆ Eˇ

φ (Ei )σD (Ei ) dEi ,

(I.1)

where N is the atom number density, Eˆ is the maximum energy of the incoming particle, Eˇ is the minimum energy of the incoming particle, φ (Ei ) is the energy dependent particle flux, and σD (Ei ) is the energy dependent displacement cross section:

σD (Ei ) =

Tˆ Tˇ

σ (Ei )ν (T ) dT ,

(I.2)

where Tˆ is the maximum energy transferred in a collision of a particle of energy Ei and a lattice atom, Tˇ is the minimum energy transferred in a collision of a particle of energy Ei and a lattice atom, σ (Ei , T ) is the cross section for the collision of a particle of energy Ei that results in a transfer of energy T to the struck atom, ν (T ) is the number of displacements per primary knock-on atom. So, ultimately, we want to determine: R=N

Eˆ Tˆ Eˇ

Tˇ

φ (Ei )σ (Ei , T )ν (T ) dT dEi .

(I.3)

The two key variables in this equation are σ (Ei , T ) and ν (T ). The term σ (Ei , T ) describes the transfer of energy from the incoming particle to the first atom it encounters in the target, the primary knock-on atom (PKA). Determination of this quantity is the goal of Chap. 1. The second quantity is ν (T ), the total number of displacements that the PKA goes on to make in the solid, and its determination is described in detail in Chap. 2. Taken together, they describe the total number of displacements caused by an incoming particle of energy Ei , and Eq. (I.3) accounts for the energy distribution of the incoming particles. The result is the total number of displacements in the target from a flux of particles with a known energy distribution. We will return to this equation often, as it is the essence of the quantification of radiation damage in solids.

References 1. Butler D (2004) Nuclear Power’s New Dawn. Nature 429:238–240 2. Greenwood LR (1994) J Nucl Mater 216:29–44

Contents

Movies accompanying the text are located at: www.sitemaker.umich.edu/was.

Part I Radiation Damage 1

The Radiation Damage Event . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Neutron–Nucleus Interactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.1 Elastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.2 Inelastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.3 (n, 2n) Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.4 (n, γ ) Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Interactions Between Ions and Atoms . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Interatomic Potentials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 Collision Kinematics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Ionization Collisions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 Energy Loss Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.2 Range Calculations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2

The Displacement of Atoms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73 2.1 Elementary Displacement Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 73 2.1.1 Displacement Probability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74 2.1.2 The Kinchin and Pease Model for Atom Displacements . . . 75 2.1.3 The Displacement Energy . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78 2.1.4 The Electron Energy Loss Limit . . . . . . . . . . . . . . . . . . . . . . . 83 2.2 Modifications to the K–P Displacement Model . . . . . . . . . . . . . . . . . . 85 2.2.1 Consideration of Ed in the Energy Balance . . . . . . . . . . . . . . 85 2.2.2 Realistic Energy Transfer Cross Sections . . . . . . . . . . . . . . . 86 2.2.3 Energy Loss by Electronic Excitation . . . . . . . . . . . . . . . . . . 87 2.2.4 Effects of Crystallinity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 2.3 The Displacement Cross Section . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105 2.3.1 Elastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 106 2.3.2 Inelastic Scattering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 2.3.3 (n, 2n) and (n, γ ) Displacements . . . . . . . . . . . . . . . . . . . . . . . 107 2.3.4 Modifications to the K–P Model and Total Displacement Cross Section . . . . . . . . . . . . . . . . . . 108

3 4 4 11 14 15 17 17 24 44 44 57 66 68 71

XVI

Contents

2.4 Displacement Rates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 109 2.5 Correlation of Property Changes and Irradiation Dose . . . . . . . . . . . . 113 2.6 Displacements from Charged Particle Irradiation . . . . . . . . . . . . . . . . 115 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 119 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 121 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 3

The Damage Cascade . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 3.1 Displacement Mean Free Path . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 125 3.2 Primary Recoil Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 126 3.3 Cascade Damage Energy and Cascade Volume . . . . . . . . . . . . . . . . . . 131 3.4 Computer Simulations of Radiation Damage . . . . . . . . . . . . . . . . . . . . 133 3.4.1 Binary Collision Approximation (BCA) Method . . . . . . . . . 133 3.4.2 Molecular Dynamics (MD) Method . . . . . . . . . . . . . . . . . . . . 136 3.4.3 Kinetic Monte Carlo (KMC) Method . . . . . . . . . . . . . . . . . . . 138 3.5 Stages of Cascade Development . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 140 3.6 Behavior of Defects within the Cascade . . . . . . . . . . . . . . . . . . . . . . . . 143 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 152 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 153 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 154

4

Point Defect Formation and Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . 155 4.1 Properties of Irradiation-Induced Defects . . . . . . . . . . . . . . . . . . . . . . . 155 4.1.1 Interstitials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 155 4.1.2 Multiple Interstitials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 160 4.1.3 Interstitial–Impurity Complexes . . . . . . . . . . . . . . . . . . . . . . . 161 4.1.4 Vacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 162 4.1.5 Multiple Vacancies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 162 4.1.6 Solute–Defect and Impurity–Defect Clusters . . . . . . . . . . . . 162 4.2 Thermodynamics of Point Defect Formation . . . . . . . . . . . . . . . . . . . . 164 4.3 Diffusion of Point Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167 4.3.1 Macroscopic Description of Diffusion . . . . . . . . . . . . . . . . . . 168 4.3.2 Mechanisms of Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . 169 4.3.3 Microscopic Description of Diffusion . . . . . . . . . . . . . . . . . . 172 4.3.4 Jump Frequency, Γ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 174 4.3.5 Jump Frequency, ω . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 176 4.3.6 Equations for D . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 177 4.4 Correlated Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 180 4.5 Diffusion in Multicomponent Systems . . . . . . . . . . . . . . . . . . . . . . . . . 182 4.6 Diffusion along High Diffusivity Paths . . . . . . . . . . . . . . . . . . . . . . . . . 184 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 187 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 188 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 190

Contents

5

XVII

Radiation-Enhanced and Diffusion Defect Reaction Rate Theory . . . 191 5.1 Point Defect Balance Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 192 5.1.1 Case 1: Low Temperature, Low Sink Density . . . . . . . . . . . . 194 5.1.2 Case 2: Low Temperature, Intermediate Sink Density . . . . . 196 5.1.3 Case 3: Low Temperature, High Sink Density . . . . . . . . . . . 197 5.1.4 Case 4: High Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . . . 199 5.1.5 Properties of the Point Defect Balance Equations . . . . . . . . . 201 5.1.6 Deficiencies of the Simple Point Defect Balance Model . . . 203 5.2 Radiation-Enhanced Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 203 5.3 Defect Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 206 5.3.1 Defect Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 209 5.3.2 Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 5.3.3 Loss to Sinks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 210 5.3.4 Sink Strengths . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4 Reaction Rate-Controlled Processes . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4.1 Defect–Void Interaction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 211 5.4.2 Defect–Dislocation Interaction . . . . . . . . . . . . . . . . . . . . . . . . 212 5.5 Diffusion-Limited Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 212 5.5.1 Defect–Void Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 213 5.5.2 Defect–Dislocation Reactions . . . . . . . . . . . . . . . . . . . . . . . . . 215 5.6 Mixed Rate Control . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 217 5.7 Defect–Grain Boundary Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . 218 5.8 Coherent Precipitates and Solutes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 219 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 222 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 223 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 227

Part II Physical Effects of Radiation Damage 6

Radiation-Induced Segregation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 231 6.1 Radiation-Induced Segregation in Concentrated Binary Alloys . . . . . 233 6.1.1 Solution to the Coupled Partial Differential Equations . . . . . 239 6.1.2 Interstitial Binding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 240 6.1.3 Solute Size Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 241 6.1.4 Effect of Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 242 6.1.5 Effect of Dose Rate . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 245 6.2 RIS in Ternary Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 246 6.3 Effect of Local Composition Changes on RIS . . . . . . . . . . . . . . . . . . . 250 6.4 Effect of Solutes on RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 253 6.5 Examples of RIS in Austenitic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . 256 6.6 RIS in Ferritic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 259 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 263 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 264 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 265

XVIII

Contents

7

Dislocation Microstructure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 267 7.1 Dislocation Lines . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 267 7.1.1 Dislocation Motion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 270 7.1.2 Description of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . 274 7.1.3 Displacements, Strains and Stresses . . . . . . . . . . . . . . . . . . . . 276 7.1.4 Energy of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 280 7.1.5 Line Tension of a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . 281 7.1.6 Forces on a Dislocation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 283 7.1.7 Interactions Between Dislocations . . . . . . . . . . . . . . . . . . . . . 289 7.1.8 Extended Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 292 7.1.9 Kinks and Jogs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 294 7.2 Faulted Loops and Stacking Fault Tetrahedra . . . . . . . . . . . . . . . . . . . 294 7.3 Defect Clusters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 298 7.3.1 Fraction of Defects Forming Clusters . . . . . . . . . . . . . . . . . . 298 7.3.2 Types of Clusters . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 300 7.3.3 Cluster Mobility . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 304 7.4 Extended Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 306 7.5 Effective Defect Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 311 7.6 Nucleation and Growth of Dislocation Loops . . . . . . . . . . . . . . . . . . . 313 7.6.1 Loop Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313 7.6.2 Clustering Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 319 7.6.3 Production Bias-Driven Cluster Nucleation . . . . . . . . . . . . . . 321 7.7 Dislocation Loop Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 325 7.8 Recovery . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 329 7.9 Evolution of the Interstitial Loop Microstructure . . . . . . . . . . . . . . . . 332 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 335 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 338 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 341

8

Irradiation-Induced Voids and Bubbles . . . . . . . . . . . . . . . . . . . . . . . . . 343 8.1 Void Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 343 8.1.1 Equilibrium Void Size Distribution . . . . . . . . . . . . . . . . . . . . 345 8.1.2 Void Nucleation Rate . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 348 8.1.3 Effect of Inert Gas . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 355 8.1.4 Void Nucleation with Production Bias . . . . . . . . . . . . . . . . . . 362 8.2 Void Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 365 8.2.1 Defect Absorption Rates and Concentrations at Sink Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 366 8.2.2 Point Defect Balances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 370 8.3 Void Growth Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 372 8.3.1 Temperature Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . 377 8.3.2 Dose Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 380 8.3.3 Role of Dislocations as Biased Sinks . . . . . . . . . . . . . . . . . . . 384 8.3.4 Dose Rate Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 385 8.3.5 Irradiation Variable Shifts . . . . . . . . . . . . . . . . . . . . . . . . . . . . 388

Contents

XIX

8.3.6 Stress Dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 393 8.3.7 Effect of RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 397 8.3.8 Effect of Production Bias . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 399 8.3.9 Void Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 402 8.3.10 Effect of Microstructure and Composition . . . . . . . . . . . . . . 404 8.3.11 Effect of Reactor Operating History . . . . . . . . . . . . . . . . . . . . 409 8.4 Bubble Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 415 8.4.1 Bubble Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 415 8.4.2 Growth Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 418 8.4.3 Bubble Growth by Dislocation Loop Punching . . . . . . . . . . . 421 8.4.4 Bubble Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 422 8.4.5 Helium Production . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 423 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 423 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 427 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 430 9

Phase Stability Under Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 433 9.1 Radiation-Induced Segregation and Radiation-Induced Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . 433 9.2 Recoil Dissolution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 436 9.3 Radiation Disordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 445 9.4 Incoherent Precipitate Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 450 9.5 Coherent Precipitate Nucleation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 455 9.6 Metastable Phases . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 460 9.6.1 Order–Disorder Transformations . . . . . . . . . . . . . . . . . . . . . . 461 9.6.2 Crystal Structure Transformations . . . . . . . . . . . . . . . . . . . . . 461 9.6.3 Quasicrystal Formation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 9.7 Amorphization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 463 9.7.1 Heat of Compound Formation and Crystal Structure Differences . . . . . . . . . . . . . . . . . . . . . . 464 9.7.2 Solubility Range of Compounds and Critical Defect Density . . . . . . . . . . . . . . . . . . . . . . . . . . . 467 9.7.3 Thermodynamics and Kinetics of Amorphization . . . . . . . . 470 9.8 Phase Stability in Reactor Core Component Alloys . . . . . . . . . . . . . . 480 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 484 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 487 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 488

10 Unique Effects of Ion Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 491 10.1 Ion Irradiation Techniques . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 491 10.2 Composition Changes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 494 10.2.1 Sputtering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 495 10.2.2 Gibbsian Adsorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 501 10.2.3 Recoil Implantation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 503 10.2.4 Cascade (Isotropic, Displacement) Mixing . . . . . . . . . . . . . . 506

XX

Contents

10.2.5 Combination of Processes Affecting Surface Compositional Changes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 518 10.2.6 Implant Re-Distribution During Ion Implantation . . . . . . . . 522 10.3 Other Effects of Ion Implantation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 525 10.3.1 Grain Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 525 10.3.2 Texture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527 10.3.3 Dislocation Microstructure . . . . . . . . . . . . . . . . . . . . . . . . . . . 528 10.4 High Dose Gas Loading: Blistering and Exfoilation . . . . . . . . . . . . . . 530 10.5 Solid Phases and Inert Gas Bubble Lattices . . . . . . . . . . . . . . . . . . . . . 535 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 537 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 540 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 543 11 Simulation of Neutron Irradiation Effects with Ions . . . . . . . . . . . . . . 545 11.1 Motivation for Using Ion Irradiation as a Surrogate for Neutron Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 545 11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation 547 11.3 Particle Type Dependence of RIS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 550 11.4 Advantages and Disadvantages of the Various Particle Types . . . . . . 557 11.4.1 Electrons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 558 11.4.2 Heavy Ions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 562 11.4.3 Protons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 564 11.5 Irradiation Parameters for Particle Irradiations . . . . . . . . . . . . . . . . . . 565 11.6 Emulation of Neutron Irradiation Damage with Proton Irradiation . . 567 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 574 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 575 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 576 Part III Mechanical Effects of Radiation Damage 12 Irradiation Hardening and Deformation . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1 Elastic and Plastic Deformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1.1 Elasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 581 12.1.2 Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 587 12.1.3 Tension Test . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 589 12.1.4 Yield Strength . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 592 12.2 Irradiation Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 594 12.2.1 Source Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 595 12.2.2 Friction Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 597 12.2.3 Superposition of Hardening Mechanisms . . . . . . . . . . . . . . . 606 12.2.4 Hardening in Polycrystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . 612 12.2.5 Saturation of Irradiation Hardening . . . . . . . . . . . . . . . . . . . . 613 12.2.6 Comparison of Measured and Predicted Hardening . . . . . . . 617 12.2.7 Radiation Anneal Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . 620

Contents

XXI

12.2.8 The Correlation Between Hardness and Yield Strength . . . . 622 12.3 Deformation in Irradiated Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 626 12.3.1 Deformation Mechanism Maps . . . . . . . . . . . . . . . . . . . . . . . . 630 12.3.2 Localized Deformation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 632 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 636 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 638 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 640 13 Fracture and Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 643 13.1 Types of Fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 643 13.2 The Cohesive Strength of Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 644 13.3 Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 647 13.4 Fracture Mechanics Tests . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 653 13.5 Elastic-Plastic Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . 655 13.6 Brittle Fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 658 13.7 Irradiation-Induced Embrittlement in Ferritic Steels . . . . . . . . . . . . . 664 13.7.1 Notched Bar Impact Testing . . . . . . . . . . . . . . . . . . . . . . . . . . 664 13.7.2 DBTT and Reduction in the Upper Shelf Energy . . . . . . . . . 666 13.7.3 Master Curve Approach . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 669 13.7.4 Factors Affecting the Degree of Embrittlement . . . . . . . . . . . 673 13.7.5 Embrittlement of Ferritic-Martensitic Steels . . . . . . . . . . . . . 677 13.7.6 Annealing and Re-Irradiation . . . . . . . . . . . . . . . . . . . . . . . . . 678 13.7.7 Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 679 13.8 Fracture and Fatigue of Austenitic Alloys at Low to Intermediate Temperatures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 685 13.8.1 Effect of Irradiation on Fracture Toughness . . . . . . . . . . . . . 686 13.8.2 Effect of Irradiation on Fatigue . . . . . . . . . . . . . . . . . . . . . . . . 689 13.9 High-Temperature Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 690 13.9.1 Grain Boundary Voids and Bubbles . . . . . . . . . . . . . . . . . . . . 692 13.9.2 Grain Boundary Sliding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 697 13.9.3 Grain Boundary Crack Growth . . . . . . . . . . . . . . . . . . . . . . . . 700 13.9.4 Fracture Mechanism Maps . . . . . . . . . . . . . . . . . . . . . . . . . . . 703 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 703 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 705 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 707 14 Irradiation Creep and Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 711 14.1 Thermal Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 712 14.1.1 Dislocation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 716 14.1.2 Diffusional Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 723 14.2 Irradiation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 725 14.2.1 Stress-Induced Preferential Nucleation of Loops (SIPN) . . . 726 14.2.2 Stress-Induced Preferential Absorption (SIPA) . . . . . . . . . . . 729 14.2.3 Climb and Glide due to Preferential Absorption (PAG) . . . . 731 14.2.4 Climb and Glide Driven by Dislocation Bias . . . . . . . . . . . . 733

XXII

Contents

14.2.5 Transient Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 734 14.2.6 Loop Unfaulting . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 738 14.2.7 Recovery Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 739 14.2.8 Diffusional Creep: Why There is no Effect of Irradiation . . 740 14.2.9 Comparison of Theory with Creep Data . . . . . . . . . . . . . . . . 741 14.2.10 Irradiation-Modified Deformation Mechanism Map . . . . . . . 744 14.3 Irradiation Growth and Creep in Zirconium Alloys . . . . . . . . . . . . . . . 746 14.3.1 Microstructure of Irradiated Zirconium Alloys . . . . . . . . . . . 747 14.3.2 Irradiation Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 750 14.3.3 Irradiation Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 753 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 758 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 760 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 762 15 Environmentally Assisted Cracking of Irradiated Metals and Alloys . 765 15.1 Stress Corrosion Cracking: A Tutorial . . . . . . . . . . . . . . . . . . . . . . . . . 768 15.1.1 SCC Tests . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 770 15.1.2 SCC Processes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 772 15.1.3 Metallurgical Condition . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 774 15.1.4 Crack Initiation and Crack Propagation . . . . . . . . . . . . . . . . . 774 15.1.5 Mechanisms of Stress Corrosion Cracking . . . . . . . . . . . . . . 783 15.1.6 Predictive Model for Crack Propagation . . . . . . . . . . . . . . . . 786 15.1.7 Mechanical Fracture Models . . . . . . . . . . . . . . . . . . . . . . . . . . 788 15.1.8 Corrosion Fatigue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 790 15.1.9 Hydrogen Embrittlement . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 790 15.2 Effects of Irradiation on Water Chemistry . . . . . . . . . . . . . . . . . . . . . . 791 15.2.1 Radiolysis and its Effect on Corrosion Potential . . . . . . . . . . 791 15.2.2 Effect of Corrosion Potential on IASCC . . . . . . . . . . . . . . . . 794 15.3 Service and Laboratory Observations of Irradiation Effects on SCC . 797 15.3.1 Austenitic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 797 15.3.2 Ferritic Alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 802 15.4 Mechanisms of IASCC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 805 15.4.1 Grain Boundary Chromium Depletion . . . . . . . . . . . . . . . . . . 805 15.4.2 Irradiation Hardening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 806 15.4.3 Deformation Mode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 807 15.4.4 Selective Internal Oxidation . . . . . . . . . . . . . . . . . . . . . . . . . . 809 15.4.5 Irradiation-Induced Creep . . . . . . . . . . . . . . . . . . . . . . . . . . . . 809 Nomenclature . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 809 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 811 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 812 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 815

Part I

Radiation Damage

1 The Radiation Damage Event

The radiation damage event is defined as the transfer of energy from an incident projectile to the solid and the resulting distribution of target atoms after completion of the event. The radiation damage event is actually composed of several distinct processes. These processes and their order of occurrence are as follows: 1. The interaction of an energetic incident particle with a lattice atom 2. The transfer of kinetic energy to the lattice atom giving birth to a primary knockon atom (PKA) 3. The displacement of the atom from its lattice site 4. The passage of the displaced atom through the lattice and the accompanying creation of additional knock-on atoms 5. The production of a displacement cascade (collection of point defects created by the PKA) 6. The termination of the PKA as an interstitial The radiation damage event is concluded when the PKA comes to rest in the lattice as an interstitial. The result of a radiation damage event is the creation of a collection of point defects (vacancies and interstitials) and clusters of these defects in the crystal lattice. It is worth noting that this entire chain of events consumes only about 10−11 s (see Table 1.1). Subsequent events involving the migration of the point defects and defect clusters and additional clustering or dissolution of the clusters are classified as radiation damage effects. What we first need to know in order to understand and quantify radiation damage, is how to describe the interaction between a particle and a solid that produces displacements, and later on, how to quantify this process. The most simple model is one that approximates the event as colliding hard spheres with displacement occurring when the transferred energy is high enough to knock the struck atom off its lattice site. In addition to energy transfer by hard-sphere collisions, the moving atom loses energy by interactions with electrons, the Coulomb field of nearby atoms, the periodicity of the crystalline lattice, etc. The problem is reduced to the following. If we can describe the energy-dependent flux of the incident particle and the energy transfer cross sections (probabilities) for collisions between atoms, then we can quantify the PKA production in a differential energy range and utilize this to determine the number of displaced atoms. In this chapter, we will concentrate on quantifying the energy transferred between interacting bodies as well as describing the energy transfer cross section. We

4

1 The Radiation Damage Event

Table 1.1. Approximate time-scale for the production of defects in irradiated metals (from [1]) Time (s)

Event

Result

10−18

Energy transfer from the incident particle Displacement of lattice atoms by the PKA Energy dissipation, spontaneous recombination and clustering

Creation of a primary knock-on atom (PKA) Displacement cascade

10−13 10−11 > 10−8

Defect reactions by thermal migration

Stable Frenkel pairs (single interstitial atoms (SIA) and vacancies) and defect clusters SIA and vacancy recombination, clustering, trapping, defect emission

will begin with neutron–nucleus reactions since the neutrality of the neutron makes the interaction particularly straightforward. Following creation of the PKA, subsequent interactions occur between atoms, and the positive charge of the nucleus and the negative charge of the electron cloud become important in understanding how atoms interact. In fact, atom–atom interaction is the low-energy limit of ion–atom interactions that occur in reactor cores and via ion irradiation using accelerators over a wide energy range and can lead to the last type of interaction: ionization collisions.

1.1 Neutron–Nucleus Interactions 1.1.1 Elastic Scattering By virtue of their electrical neutrality, elastic collisions between neutrons and nuclei can be represented as colliding hard spheres. When neutrons pass through a solid, there is a finite probability that they will collide with a lattice atom, imparting a recoil energy to the struck atom. This probability is defined by the double differential scattering cross section (in energy and angle), σs (Ei , Ef , Ω ), where, Ei and Ef are the incident and final energies and Ω is the solid angle into which the neutron is scattered. We are often only interested in the scattering probability as a function of Ei and the scattering angle. The single differential scattering cross section is:

σs (Ei , Ω ) =

σs (Ei , Ef , Ω ) dEf .

(1.1)

The total scattering probability for neutrons of energy Ei is:

σs (Ei ) =

σs (Ei , Ω ) dΩ .

(1.2)

1.1 Neutron–Nucleus Interactions

5

In the study of irradiation effects, we are interested in the behavior of the struck atom. So we are seeking σs (Ei , T ); the energy transfer cross section, or the probability that a neutron of energy Ei elastically scattering against an atom of mass M, will impart a recoil energy T to the struck atom. But first it is necessary to find T in terms of the neutron energy and the scattering angle. To do this, let us consider the dynamics of binary elastic collisions in the center-of-mass and laboratory frames. Figure 1.1a shows the trajectories of a neutron and the target nucleus before and after scattering, as seen from both the laboratory reference system and the center-ofmass system. The easiest way to obtain a relationship between the incident neutron energy, scattering angle and transferred energy is to analyze the dynamics of the collision in the center-of-mass (CM) system. When the collision is viewed in the center-of-mass system, the recoiling particles appear to move away from each other in opposite directions. Momentum conservation along the axes of approach and departure yield: c m − VcM = 0 c m − Vc M = 0 ,

(1.3)

and conservation of kinetic energy requires that: 1 2 1 1 1 2 mc + MVc2 = m2 c + MVc . 2 2 2 2 Using Eq. (1.3) to eliminate c and c , we get: 2 2 M M 1 1 1 1 2 m m + M Vc = + M Vc2 . 2 m 2 2 m 2

(1.4)

(1.5)

Therefore, Vc = Vc , and hence, c = c .

(1.6)

Since the target nucleus is at rest in the lab system and moving to the left with speed Vc in the CM system, the CM system itself must be moving to the right relative to the lab system with the same speed, Vc . Thus, if we use VCM to denote the speed of the CM system relative to the laboratory system, the magnitudes of VCM and Vc are the same (but opposite in direction). This can be restated as follows: c = − VCM = − Vc , and using Eq. (1.3), we find that: m VCM = . M+m

(1.7)

(1.8)

Recall that we want to relate T , the energy transferred to the struck atom, to φ , the scattering angle in the CM system. Using vector addition we can relate the recoil

6

1 The Radiation Damage Event

Fig. 1.1. Vector velocities (a) in the laboratory and center-of-mass (CM) systems, and (b) composite diagram relating velocities in the two systems

target nucleus velocity in the lab system, V , to φ as shown in Fig. 1.1b, which is a composite of the interaction in the lab and CM systems shown in Fig. 1.1a. Using the law of cosines: 2 V2 = VCM + Vc2 − 2VCMVc cos φ ,

and re-writing the velocities in Eq. (1.9) in terms of energy gives: 2 m 2T 2Ei 2m 2 2 V = , VCM = , and Vc2 = 2 Em , M m m+M M

(1.9)

1.1 Neutron–Nucleus Interactions

and substituting these expressions into Eq. (1.9) gives: m m mM 1/2 E + Em − 2 cos φ , T= Ei Em 2 i M m+M (m + M) or T = η1 η2 Ei +

η1 1/2 Em − 2η1 Ei Em cos φ , η2

7

(1.10a)

(1.10b)

where η1 = m/(m + M) and η2 = M/(m + M). Since we want to find the energy transferred, T as a function of initial energy to eliminate and scattering angle only, we use the relationship between Ei and Em Em . From Eqs. (1.7) and (1.8), we know that: m M c = − = . (1.11) m+M m+M Writing Eq. (1.11) in terms of energy gives: 2 M = Ei = η22 Ei . Em m+M

(1.12)

Substituting into Eq. (1.10b) and simplifying gives:

γ T = Ei (1 − cos φ ) , 2 where we define 4mM 4A γ= = , 2 (M + m) (1 + A)2

(1.13)

(1.14)

where 1 = m and A = M. Hence, T depends upon only one unknown, φ . Note the angular dependence of T on φ as shown in Fig. 1.2. The energy transferred rises from 0 at φ = 0 to a maximum of γ Ei at φ = π , or Tmin = Tˇ = 0 and Tmax = Tˆ = 0. That is, the energy transferred is a maximum when the particle backscatters and is a minimum when it misses the target, resulting in no change in course (φ = 0).

Example 1.1. For a neutron incident on a hydrogen atom, Tˆn-H /Ei = 1.0. But for a neutron incident on a uranium atom, Tˆn-U /Ei = 0.017. Conversely, comparing the interaction of an iron atom with 100 keV Xe+ ions or electrons, the value of γ for the Xe–Fe interaction is 0.83, yielding a Tˆ of 83,000 eV. However, the value of γ for e− –Fe interaction is 0.00004, giving a Tˆ of only 4 eV, which, as we will see in Chap. 2, is not enough to displace an iron atom from its lattice site. The scattering angles in the lab system for the incident particle (θ ) and the struck atom (α ) can be written in terms of the scattering angle in the center-

8

1 The Radiation Damage Event

Fig. 1.2. Energy transfer as a function of center-of-mass scattering angle

of-mass system (φ ) using the vector diagram in Fig. 1.1b. Applying the law of sines to Fig. 1.1b for the scattered particle: = c , sin(π − θ ) sin θ where c is given by Eqs. (1.6) and (1.7): −1 , c = VCM VCM and using Eq. (1.8), we have: c = VCM

M . m

Applying the law of cosines to the same triangle gives: 2 2 2 = c + VCM − 2VCM c cos(π − φ ) ,

and combining the last three equations to express θ as a function of φ yields: tan θ =

(M/m) sin φ . 1 + (M/m) cos φ

1.1 Neutron–Nucleus Interactions

9

Fig. 1.3. Scattering into the solid angular element dΩ defined by dA/r2

Applying the law of sines to the vector diagram in Fig. 1.1b for the struck atom gives: V Vc = , sin α sin φ and combining this result with Eqs. (1.6) and (1.9) where the energies are written in terms of velocities gives: tan α =

sin φ . 1 − cos φ

We are still interested in obtaining the probability that a given T will be imparted to the recoil atom. This depends on the differential cross section. We define σs (Ei , φ ) dΩ as the probability of a collision that scatters the incident particle into a center-of-mass angle in the range (φ , dΩ ) where dΩ is an element of solid angle about the scattering direction φ . Since differential probabilities written in transformed variables are equivalent, σs (Ei , φ ) can be written in terms of CM variables:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ .

(1.15)

Using Fig. 1.3 to relate dΩ to dφ , we have by definition: dΩ = dA/r2 ,

(1.16)

and from Fig. 1.4, we have: dΩ =

r dφ (2π r sin φ ) = 2π sin φ dφ . r2

(1.17)

Substituting Eq. (1.17) into Eq. (1.15) yields:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ = 2πσs (Ei , φ ) sin φ dφ .

(1.18)

10

1 The Radiation Damage Event Fig. 1.4. The solid angle dΩ subtended at the scattering angle φ by the incremental angle dφ

And since T = γ2 Ei (1 − cos φ ) then dT = 2γ Ei sin φ dφ , then we have:

σs (Ei , T ) =

4π σs (Ei , φ ) . γ Ei

(1.19)

Figure 1.5 shows the difference in the differential scattering cross section in units of area per unit solid angle vs. area per unit angle as in Eq. (1.18). Although the number of atoms scattered through an angle increment dφ about φ = π /2 is greater than that through an angular increment dφ about φ = 0 or π (Fig. 1.5a), the number intercepting the spherical surface per unit of solid angle is constant over all angles, φ (Fig. 1.5b). Hence dT / dφ varies in a sinusoidal manner with φ but dT / dΩ is independent of φ . Using Eqs. (1.2) and (1.18), the total elastic scattering cross section is:

σs (Ei ) =

σs (Ei , φ ) dΩ = 2π

σs (Ei , φ ) sin φ dφ .

Fig. 1.5. Isotropic differential scattering cross sections in units of (a) area per unit scattering angle and (b) area per unit solid angle

1.1 Neutron–Nucleus Interactions

11

If we assume that elastic scattering in the CM system is independent of scattering angle (i.e., scattering is isotropic), Fig. 1.6, then:

σs (Ei ) =

σs (Ei , φ ) dΩ = 2πσs (Ei , φ )

sin φ dφ = 4πσs (Ei , φ )

(1.20)

and

σs (Ei , T ) =

σs (Ei ) , γ Ei

(1.21)

which is independent of T ! That is, σs (Ei , T ), the probability that a neutron of energy Ei , elastically scattering against an atom of mass M, will impart a recoil energy T to the struck atom does not depend on the recoil energy. Now the average recoil energy can be calculated: Tˆ

Tˆ γ Ei Tˇ + Tˆ ˇ T σs (Ei , T ) dT T¯ = T ˆ ≈ = . = T 2 2 2 Tˇ σs (Ei , T ) dT

(1.22)

Applying Eq. (1.22) to the case of a 1 MeV neutron incident on elements of varying mass, we have the following: 1 MeV n on C: γ = 0.28 1 MeV n on Fe: γ = 0.069 1 MeV n on U: γ = 0.017

T¯ = 0.14 MeV T¯ = 0.035 MeV T¯ = 0.009 MeV

In addition to the elastic scattering just discussed, we can have energy transfer by inelastic scattering, (n, 2n) reactions and (n, γ ) reactions. The first two reactions become important above neutron energies of about 1.0 and 8.0 MeV, respectively, while the latter occurs at thermal neutron energies in 235 U. 1.1.2 Inelastic Scattering Inelastic scattering is characterized by a reaction in which the emitted particle is experimentally the same as the captured particle, but there is a loss of kinetic energy in the system. The energy is found in the excitation energy of the product nucleus, ∗ ∗ e.g., N14 (p, p’)N14 or C14 (n, n’)C14 . The differences in the energies of groups of scattered particles correspond to the energy separations of excited levels in the product nucleus: Q = ∑ KE f − ∑ KEi = ∑ M f c2 − ∑ Mi c2 . f

i

f

i

In an inelastic collision, a neutron is absorbed by the nucleus, forming a compound nucleus, which emits a neutron and a γ -ray. There may be more than one γ emitted and the nucleus may remain in an excited state during the course of an interaction. The inelastic scattering cross section can be divided into resolved and unresolved

12

1 The Radiation Damage Event

Fig. 1.6. Differential elastic scattering cross sections for C12 at 0.5 MeV and 14 MeV neutrons as a function of the cosine of the center-of-mass scattering angle (from [2])

resonance components [3]. For a given resonance ( jth resonance) of the target nucleus, the scattering cross section will be a function of Q j , the γ decay energy of the residual nucleus that is always negative. Analogous to Eq. (1.15) we can write differential equalities σs j (Ei , Q j , T ) dT = σs j (Ei , Q j , φ ) dΩ , so that:

σs j (Ei , Q j , T ) = σs j (Ei , Q j , φ ) 2π sin φ

dφ . dT

(1.23)

However, the expression for T in Eq. (1.13) is not valid for inelastic collisions since kinetic energy is not conserved. Instead we focus on the conservation of total energy. If the target nucleus M is at rest in the lab system and the particle m has energy Ei , then the energy balance in CM coordinates is: M Ei + Q j = Em + EM , M+m

(1.24)

and EM are the kinetic energies in CM where Q j is the reaction energy and Em coordinates of the exit particle and nucleus, respectively. In order that momentum is conserved: = MEM , mEm

(1.25)

and combining Eq. (1.24) with Eq. (1.25) (assuming that the masses of the projectile and target are unchanged after the reaction), yields: M M Ei Em = Qj + M+m M+m

1.1 Neutron–Nucleus Interactions

13

or Em = η2 (Q j + η2 Ei ) .

(1.26)

Recalling the general expression for T , Eq. (1.10b): T = η1 η2 Ei +

η1 172 E − 2η1 Ei Em cos φ , η2 m

from Eq. (1.26) yields and substituting in for Em

Qj γ γ A + 1 1/2 T (Ei , Q j , φ ) = Ei − . cos φ + Ei Ei + Q j 2 2 A A+1

(1.27)

Now, the expression for dT / dφ becomes:

Q j A + 1 1/2 dT (Ei , Q j , φ ) γ = Ei 1 + sin φ . dφ 2 Ei A

(1.28)

Note that in the case of elastic collisions, Q j = 0 and Eq. (1.27) reduces to Eq. (1.13). If we now assume that inelastic scattering is isotropic in the CM system, then we have:

σs j (Ei , Q j ) =

σs j (Ei , Q j , φ ) dΩ = 4πσs j (Ei , Q j , φ ) .

(1.29)

Substituting Eqs. (1.28) and (1.29) into (1.23) yields:

σs j (Ei , Q j , T ) =

σs j (Ei , Q j ) . Q j A + 1 1/2 γ Ei 1 + Ei A

(1.30)

for inelastic collisions in the resolved resonance region. When the compound nucleus is excited to high enough energies, the resonance levels overlap and are no longer individually distinguishable. The inelastic scattering cross section is treated as a continuum and is described by an evaporation model [3] with: ) f (Ei , Em σis Ei , Em , T = σis (Ei ) , and 1 1/2 Ei Em 4 A+1 E max ) m f (Ei , Em σis (Ei , T ) = σis (Ei ) dEm , (1.31) 1 1/2 0 Ei Em 4 A+1 ) is a distribution function for the energy E of the scattered neutron where f (Ei , Em m in the CM system that represents the probability that a neutron is evaporated from the moving compound nucleus, whose value in the CM system is a Maxwellian of

14

1 The Radiation Damage Event

nuclear temperature ED = kT : E f Ei , Em = m e(−Em /ED ) , I (Ei ) and

I (Ei ) = ED2

(1.32)

max max /E Em −Em D 1− 1+ e , ED

(1.33)

is a normalization factor such that E max m 0

dEm = 1 . f Ei , Em

(1.34)

is given by Eq. (1.26) with Q = Q , the lowest energy The maximum value of Em 1 is zero. level, and the minimum value of Em

1.1.3 (n, 2n) Reactions Reactions such as the (n, 2n) reaction are important in radiation effects since they produce additional neutrons that can either cause damage or transmutation reactions in components of interest. Following the 2n model, which is based on work by Odette [4] and Segev [5], a second neutron can only be emitted if the residual excitation of the nucleus after emission of the first neutron exceeds the binding energy of a neutron in the mass-M nuclide. The recoil energy after emission of the first neutron is taken to be the average value (cos φ = 0 in Eq. (1.10b)) and is shown in Fig. 1.7a in the lab system. We next analyze the second reaction (emission) in the CM system described in Fig. 1.7b. We begin by using the law of cosines to relate Vc to φ : V2 = V2 + Vc2 − 2VVc cos φ .

(1.35)

From Fig. 1.7a, we have: 1 MV 2 = T¯ 2

or V2 =

2T¯ , M

and from Fig. 1.7b we have: 1 (M − m)Vc2 = EM 2

or Vc2 =

2EM . M−m

Conservation of momentum requires: (M − m)Vc = mc ,

(1.36)

1.1 Neutron–Nucleus Interactions

15

and squaring gives: Vc2

=

m M−m

2

2 c =

2m E . (M − m)2 m

(1.37)

Substituting into the law of cosines, Eq. (1.35), gives: V2 =

2m 2m 2 ¯ 1/2 2T¯ + E T E − 2 cos φ , M (M − m)2 m (M − m)2 M m

(1.38)

is the mean recoil energy after emission of the where T¯ = η1 η2 Ei + (η1 /η2 ) Em 2 first neutron. Writing V in terms of energy gives the recoil energy following the second emission: 1 T = (M − m)V2 2 m 1/2 M−m ¯ m ¯ 1/2 Em = −2 (Em T ) cos φ T + M M−m M 1/2 1 A−1 ¯ 1 1/2 E − 2 T¯ Em = cos φ T + A A−1 m A 1/2 η1 A η1 A − 1 ¯ 1/2 T − 2 T¯ Em = Em + cos φ . (1.39) A − 1 η2 A η2

The (n, 2n) reaction cross section is a special case of the inelastic scattering cross section given in Eq. (1.31): σn,2n Ei , Em , Em , T = σn,2n (Ei )

σn,2n (Ei , T ) =

Em Em e−Em /ED e−Em /ED , I (Ei ) I (Ei , Em )

Ei −U Ei −U−E m Em e−Em /ED 0

I (Ei )

0

and

Em e−Em /ED dEm dEm , I (Ei , Em )

(1.40) max = E − U and I (E , E ) is Eq. (1.33) where I (Ei ) is given in Eq. (1.33) with Em i i m max max , and for (n, 2n) reactions, U = 0 [3]. with Em replaced by Em = Ei − U − Em

1.1.4 (n, γ ) Reactions Another class of reactions that can affect the extent of radiation damage involves photon emission. This reaction is important since the energy of the recoiling nucleus is sufficient to displace an atom. As we will see later, this type of displacement is particularly important in radiation damage in reactor pressure vessels in which the gamma flux is more comparable to the fast neutron flux than in the reactor core. Recalling the momentum and energy conservation laws of Eqs. (1.3) and (1.4) and

16

1 The Radiation Damage Event

Fig. 1.7. Vector velocities for the (n, 2n) reaction in (a) the lab system and (b) the center-ofmass system

Fig. 1.1, which for (n, γ ) reactions, Ei ∼ 0 (since these reactions occur with thermal neutrons of energy 0.025 eV), Ef ≡ 0 (since there is no scattered neutron) and Q is the equivalent of the mass difference between the initial particles and the compound nucleus. When the compound nucleus (CN) de-excites, it emits a γ -ray with this energy. Conservation of momentum says that the nucleus must recoil with momentum: (m + M)Vc =

Eγ . c

(1.41)

Note that this is an approximation since we have not subtracted the mass defect from the compound nucleus. Squaring both sides of Eq. (1.41) and dividing by 2(m + M) gives: Eγ2 1 (m + M)Vc2 = . 2 2(m + M)c2 As in the case of elastic scattering, T is given by: 2 M+m 2 T = VCM + Vc − 2VCMVc cos φ , 2 but VCM Vc so to a good estimate: Eγ2 m+M 2 T∼ = . V = c 2 2(M + m)c2 We will assume further that this value of T represents the maximum recoil energy. But since not all of Q will be emitted in a single γ -ray, we approximate the average recoil energy as half the value of the maximum recoil energy, giving: T¯ ∼ =

Eγ2 . 4(M + m)c2

(1.42)

1.2 Interactions Between Ions and Atoms

17

The radiative capture cross section is derived from the Breit–Wigner single-level formula when the target nucleus has zero intrinsic angular momentum and the compound nucleus has a neutron width Γn and a radiation width Γg , and a total width Γ , and E0 is the resonance energy and λ is the wavelength [6]:

σn,γ (Ei ) = πλ 2

ΓnΓγ . (Ei − E0 )2 + (Γ /2)2

(1.43)

Expressing Eq. (1.43) in terms of σ0 , the maximum value of the radiative cap√ ture cross section (at E = E0 ) and taking the Γn proportional to 1/λ and to E gives: E0 1 . (1.44) σn,γ (Ei ) = σ0 Ei [(Ei − E0 ) /(Γ /2)]2 + 1 Table 1.2 provides a summary of the energy transfer and the energy transfer cross sections for the various types of reactions covered in Sect. 1.1.

1.2 Interactions Between Ions and Atoms Ion–atom or atom–atom collisions are governed by interactions between the electron clouds, the electron cloud and the nucleus, and between the nuclei. These interactions are described by what are known as interatomic potentials. In order to develop descriptions of energy transfer cross sections for interactions between atoms, we need descriptions of the potential function that governs that interaction. Unfortunately, there exists no single function that describes all interactions, but rather, the nature of the interaction is a strong function of the atom energies, and hence their distance of closest approach of their nuclei. The following section provides a summary of interatomic potentials adapted from Chadderton [7]. 1.2.1 Interatomic Potentials The end product of the neutron–nuclear interaction is the creation of the primary knock-on atom with some amount of kinetic energy. This atom will, of course, make subsequent collisions with other atoms in the solid. Knowledge of the forces acting between two colliding atoms represents the most fundamental aspect of radiation damage, without which a proper description of the primary event and the ensuing defect structure is impossible. Our interest lies in the forces between like atoms, unlike atoms, or ions and atoms. The description of interactions between atoms is done using potential functions. Recall that the atoms are (usually) electrically neutral but are composed of positive and negative components that do not cancel at all points in space. It is well known that the potential energy between two point

18

1 The Radiation Damage Event

Table 1.2. Energy transfer and energy transfer cross sections for various types of neutron– nuclear collisions Type of collision

Elastic scattering

Energy transfer and energy transfer cross section

γ T = Ei (1 − cos φ ) 2

(1.13)

σs (Ei ) γ Ei

(1.21)

σs (Ei , T ) = Inelastic scattering

Qj γ γ A + 1 1/2 cos φ + T (Ei , Q j , φ ) = Ei − E i E i + Qi 2 2 A A+1 resonance region

σs, j (Ei , Q j , T ) =

σs, j (Ei , Q j )

Qj l +A γ Ei 1 + Ei A unresolved resonance region

σn,2n (Ei , T ) =

E max m

Ei −U Em e−Em /ED I (Ei ) 0 Ei −U −E

×

(n, γ )

1/2

) f (Ei , Em dEm 1 0 1/2 4 EE A+1 i m 1/2 η1 A η1 A − 1 ¯ 1/2 T¯ Em T −2 T= E + cos φ A − 1 η2 m A η2

σis (Ei , T ) = σis (Ei )

(n, 2n)

Equation in text

m

0

Em −Em /ED dEm dEm )e I (Ei , Em

Eγ2 4(M + m)c2 1 E0 σn,γ (Ei ) = σ0 Ei [(Ei − E0 )/(Γ /2)]2 + 1 T¯ ∼ =

(1.27)

(1.30)

(1.31)

(1.39)

(1.40) (1.42) (1.44)

charges of the same sign separated by a distance r is described by the well know Coulomb equation: V (r) =

ε2 , r

(1.45)

where ε is a single unit charge. However, in the case of atoms, we have a charged nucleus surrounded by an electron cloud of opposite charge. It is evident that the potential function describing the interaction between atoms is far more complicated. Even in the simplest cases, V (r) has never been determined exactly, but some simple considerations show that it must be dominated by two distinct contributions over the

1.2 Interactions Between Ions and Atoms

19

range of separation in which we are interested. Perhaps the simplest of all potential functions is the “hard-sphere” approximation. This potential is described as follows: 0 for r > r0 V (r) = (1.46) ∞ for r < r0 . This potential function describes an interaction with an infinitely sharp cut-off at the atomic radius r0 . At distances greater than this radius the interaction vanishes, while at distances less than r0 the magnitude is infinity. This description is analogous to the behavior of billiard balls and hence, the atoms in this model are described as acting as such. Clearly this is not a very realistic description of atom–atom interaction since we know that the electron shells can overlap. Figure 1.8 shows how the interatomic potential actually varies with separation. At large separation, the principal interaction is supplied by the Coulomb forces while for smaller separations, the central field repulsive force is dominant. A similar relationship applies to all crystals regardless of the nature of binding. In all cases there is a smooth curve with a minimum at the separation distance corresponding to the nearest neighbor distance in the lattice, re (also referred to as D). In describing the interaction between atoms, we will use two yardsticks for points of reference. One is the Bohr radius of the hydrogen atom, a0 = 0.053 nm, which provides a measure of the position of the atomic shells. The other is re , the spacing between nearest neighbors in the crystal (typically ∼ 0.25 nm). When r re , electrons populate the lowest energy levels (closed shells) of the individual atoms and only the outer valence shells will have empty levels. As two atoms are brought together, the valence shells begin to overlap and weak attractive forces such as van de Waals forces may develop. When a0 < r ≤ re the closed inner shells begin to overlap. Since the Pauli exclusion principle demands that some electrons change their levels, and hence move to higher energy levels, the extra energy supplied in forcing the atoms together constitutes a positive potential energy of interaction. This is known as closed shell repulsion and the potential that most accurately describes

Fig. 1.8. Variation of interatomic potential with separation, r. Coulomb forces dominate at large separations (b) and the central repulsive force dominates at small separations (a), and at intermediate distances, there is a smooth transition between the two extremes with a minimum corresponding to the equilibrium separation distance, re or D

20

1 The Radiation Damage Event

this region is the Born–Mayer potential: V (r) = A exp(−r/B) ,

(1.47)

where A and B are constants determined from the elastic moduli [8]. Although this function was first used by Born and Mayer to represent core ion repulsion in their theory of ionic crystals, it is perfectly valid for separations on the order of the equilibrium separation, re , and is useful in treatments of threshold or near-threshold collisions where the impact parameter is of the order re . When r a0 , Coulomb interaction between the nuclei dominates all other terms in V (r): V (r) =

Z1 Z2 ε 2 . r

(1.48)

At slightly larger distances, the nuclear charges are electrostatically “screened” by the space charge of the innermost electron shells that have entered the internuclear space. The potential describing this behavior is known as the screened Coulomb potential [8, 9, 10, 11, 12]: Z1 Z2 ε 2 V (r) = exp(−r/a) , (1.49) r where a =

Ca0

2/3 2/3 1/2 Z1 + Z2

or a =

Ca0 (Z1 Z2 )1/6

, C = 0.8853 and a0 is the Bohr radius

of the hydrogen atom. More generally, screening by the electron cloud is described by a screening function, χ (r) that is defined as the ratio of the actual atomic potential at a radius r to the Coulomb potential. The function of χ (r) is to moderate the Coulomb potential to describe the interaction between atoms at all separation distances. For large distances, χ (r) will tend toward zero, and at very small distances, χ (r) will tend toward unity. This is one way in which a single interatomic potential function can be used to describe all collisions. We have now described two regimes of interaction. At small separations (r a0 ) the screened Coulomb term dominates all others, with the screening effect decaying exponentially with the separation distance. In the region a0 < r ≤ re electronic interaction dominates and is best described by the Born–Mayer potential. At intermediate separations there is no satisfactory description of the nature of atomic interaction. Unfortunately, it is exactly in this region where information is needed to provide a proper analytical description of radiation damage. Nevertheless, we may make a first approximation to the total potential by summing the controlling potentials at large and small separations: V (r) =

Z1 Z2 ε 2 exp(−r/a) + A exp(−r/B) , r

(1.50)

where A = 2.58 × 10−5(Z1 Z2 )11/4 eV, B = 1.5a0 /(Z1 Z2 )1/6 are empirical formulae suggested by Brinkman [11], consistent with observed compressibilities and elastic

1.2 Interactions Between Ions and Atoms

21

moduli in the noble metals Cu, Ag and Au. Unfortunately, there is a little experimental information about the forces between metal atoms, which is our primary interest. Figure 1.9 shows that the first term dominates for small separation and the second for large. Brinkman suggested a model for the interaction between two identical atoms in which the nucleus is surrounded by a rigid charge distribution ρε and it is assumed that both atoms supply a screened Coulomb field of the same type: V (r) =

r Z 2 ε 2 −r/a 1− e . r 2a

(1.51)

This relation approaches the Coulomb repulsion as r approaches zero and changes sign √ at r = 2a, becoming a weak attractive potential with a minimum at r = a(1 + 3). However, this potential predicts a strong interaction energy at large distances and may not represent the true physical picture for metals. Brinkman formulated a new potential function: V (r) =

AZ1 Z2 ε 2 exp(−Br) . 1 − exp(−Ar)

(1.52)

Note that for small values of r the potential closely approximates the Coulomb repulsive interaction, i.e., lim V (r) →

r→∞

Z1 Z2 ε 2 , r

Fig. 1.9. Behavior of various potential functions over a range of separation distances between copper atoms

22

1 The Radiation Damage Event

and at large separation, the potential equation approximates the exponential repulsion of the Born–Mayer type: lim V (r) → AZ1 Z2 ε 2 exp(−Br) .

r→∞

1/3

The constant B is defined as B = Zeff /Ca0 , where Zeff = (Z1 Z2 )1/2 , and C is of the order 1.0 or 1.5. The constant A depends on the compressibility and bulk modulus, which depend on the overlap of closed electron shells. An empirical expression for 0.95 × 10−6 7/6 Zeff . Substituting for A, B and C (= 1.5) into Eq. (1.52) gives: A is A = a0

1/3 exp −Zeff r/1.5a0 1/2

, V (r) = 1.9 × 10−6Zeff ER (1.53) 7/6 1 − exp −0.95 × 10−6Zeff r/a0 where ER = ε 2 /2a0 is the Rydberg energy (13.6 eV). It should be noted that although the potential is a reasonably reliable function for all metals whose atomic number exceeds 25 over the range r < 0.7re , it should not be used near r = re since in the derivation it has been implicitly assumed that all interatomic distances are close to those of Cu, Ag and Au. It is therefore not a valid potential to use in calculating formation and migration energies of point defects. Two other potentials should be discussed. The first is the Firsov or Thomas– Fermi two-center potential. This potential function is an improvement over the screened Coulomb potential by virtue of the fact it takes into account the change in electron energy connected with the mutual approach of the nuclei. The potential can be written as: V (r) =

χ (r) , r

where χ (r) is the screening function. In the case of the screened Coulomb potential:

χ (r) = χB (r) and χB (r) = Z1 Z2 ε 2 exp (−r/a) , while in the Firsov potential:

1/2 1/2 2/3 r χ (r) = χTF (r/a) = χ Z1 + Z2 , a

(1.54)

(1.55)

so that we have:

Z1 Z2 ε 2 1/2 1/2 2/3 r χ Z1 + Z2 V (r) = , r a

(1.56)

1.2 Interactions Between Ions and Atoms

23

where

1/2 1/2 2/3 r χ Z1 + Z2 a is a screening function. The second potential of interest is the Thomas–Fermi–Dirac two-center potential (TFD). The Thomas–Fermi–Dirac statistical model of the atom was employed to calculate a potential from first principles. As a consequence, this potential takes into account exchange effects and places a finite boundary, defined by rb , on the spatial distribution of the electron cloud density ρε . The potential obtained for like atoms is: Z 2 ε 2 1/3 r − α Z + Λ¯ , χ Z V¯ (r) = r a

(1.57)

ε where α ∼ = 3.16 × 10−3 and Λ¯ is a set of integrals over exact single-center eleca0 tron densities. Calculations using this potential have shown that for very small separations of less than ∼ 0.3a0, V¯ (r) agrees well with other theoretical curves and with experiment, while in the range ∼ 0.3a0 to 3a0, V (r) agrees with other theoretical and experiment results better than the screened Coulomb potential or the Firsov potential [7]. In selecting the appropriate potential for a specific collision problem, the range of separation can be determined by equating the available kinetic energy to the potential and hence obtaining the smallest separation. The important interaction terms for the calculated separation can then be determined. For interactions between metal atoms at low kinetic energies, 10−1 to 103 eV, the Born–Mayer term alone is sufficient with constants given in Eq. (1.50). In cases of atom–atom collisions in the collision cascade, where energies from 103 to 105 eV are involved, an inverse power potential is extremely convenient. Such a potential can be formulated by fitting a function C/rs to one of the above potential functions over a limited range of r. For example, one can fit an inverse square (s = 2) function to the screened Coulomb potential at r = a, obtaining the same slope, ordinate and curvature. This function is [13]: 2

V (r) =

Z1 Z2 ε 2 a −1 e . r2

(1.58)

For a limited range of r, this can be used as an approximate potential. Re-writing using the expression in Eq. (1.49) for a gives: V (r) =

a 2 2ER 0 (Z1 Z2 )5/6 . e r

(1.59)

24

1 The Radiation Damage Event

A convenient alternative for numerical calculations uses the fact that hence: a 2 0 V (r) = 10 (Z1 Z2 )5/6 eV . r

2ER ∼ = 10 eV, e (1.60)

This potential also applies to heavy ion bombardment in the energy range 103 to 105 eV. In the case of light ions at high energy, such as 5 MeV protons, the simple Coulomb potential is adequate. Table 1.3 summarizes the various potential functions and their regions of applicability. But how do we go about verifying a potential function? For example, how do we determine the constants A and B in the Born–Mayer potential for a specific element? Since the Born–Mayer potential is based on small displacements from equilibrium (i.e., re ), we can obtain these constants from bulk property measurement of the solid,e.g.,compressibility, elastic moduli, etc. If we expand the potential φ (r) 2 2φ dφ d φ d r + 1/2 r2 + · · · , then the coefficient of is the as φ0 + dr 0 dr2 0 dr2 0 curvature of the energy–distance curve at r = re shown in Fig. 1.8. How then do we know that a given potential does or does not properly describe the interaction in a region of r? We can make this determination by scattering measurements or by measuring the range of ions in solids. Since V (r) describes the nature of the interaction, it will also tell us about σs (Ei ), that can be determined by scattering experiments. Also, range measurements give a good indication of how many interactions must have occurred in order to place the ion in its deposited location. Both of these sets of experiments will provide information on the adequacy of the chosen potential function to accurately describe the interaction between atoms in the solid. With some appreciation for the way in which neutral atoms or atoms and ions interact, we are now prepared to describe a collision between these species, which is in some ways very similar to, and in other ways very different from neutron–nuclear collisions. The resulting formalism will provide us with the tools to determine the energy transferred from the incident atom to the struck atom along with the energy transfer cross section. The following treatment is adapted from Thompson [13]. 1.2.2 Collision Kinematics The orbits of two colliding atoms are shown in Fig. 1.10 relative to the center of mass of the masses M1 and M2 . Particle locations are most conveniently denoted in polar coordinates (r1 , ψ ) and (r2 , ψ ) for masses M1 andM2 , respectively. The impact parameter is b, ψ is the scattering angle of the struck atom in the lab system and φ is the asymptotic scattering angle when the interparticle spacing approaches infinity. The impact parameter is defined as the distance between the asymptotic trajectories of the colliding particles as shown in Fig. 1.10. We are interested in determining the detailed orbits by expressing φ is a function of b. This result will then be used to determine the scattering cross section.

Inverse square

TFD two-center

Firsov

Brinkman II

Brinkman I

r < 0.7re

A=

Z > 25

a 2 2Er 0 (Z1 Z2 )5/6 e r

a/2 < r < 5a

0.95 × 10−6

a0 /Z 1/3

ER = Rydberg energy = 13.6 eV

(1.59)

(1.57) cloud density vanishes

rb = Radius at which the electron

(1.52)

(1.56)

7/6

Zeff

χ is screening function

a0 1/3 B = Zeff /Ca0 C∼ = 1.5

a∼ =

r r0 ∞ for r < r0 V (r) = A exp(−r/B)

Hard-sphere

Born–Mayer

Definitions

Range of applicability

Equation for V (r) =

Potential

Table 1.3. Summary of potential functions

1.2 Interactions Between Ions and Atoms 25

26

1 The Radiation Damage Event

Fig. 1.10. Collision orbits in the center-of-mass system

The radial and transverse velocity of mass M1 are r˙1 and r1 ψ˙ in polar coordinates, and the resultant velocity is (˙r12 + r12 ψ˙ 2 )1/2 . The velocity components are the same for mass M2 with the subscript 2 substituted for 1. Conservation of energy requires that the total energy of any system remain constant. The energy in the lab 1 M1 reference system is just Ei = M1 2 = ET . Recall that VCM = , and that 2 M1 + M2 the kinetic energy of the center of mass itself (in the lab system) is: M1 1 2 = ECM = (M1 + M2 )VCM Ei . 2 M1 + M2 Hence, the energy in the CM system that is available for transformation is the total kinetic energy less the motion energy of the CM system: M2 . (1.61) E = ET − ECM = Ei − ECM = Ei M 1 + M2 In an elastic collision, the sum of the potential and kinetic energies at any point in the orbit must equal the asymptotic sum of kinetic energies, so: 1 M2 1 = M1 r˙12 + r12 ψ˙ 2 + M2 r˙22 + r22 ψ˙ 2 + V (r1 + r2 ). Ei M1 + M2 2 2 (1.62) asymptotic sum of kinetic energy at any point potential energy in orbit energy

1.2 Interactions Between Ions and Atoms

Letting r = r1 + r2 be the total separation distance, and r1 = M1 r, and the energy balance of Eq. (1.62) simplifies to: M1 + M2

27

M2 r, r2 = M1 + M2

1 η Ei = μ r˙2 + r2 ψ˙ 2 + V (r) , 2

(1.63)

M2 M1 M2 and μ = is the reduced mass. M1 + M2 M1 + M2 The law of conservation of angular momentum demands that the value at any point in the orbit must equal the asymptotic value. Recall that: M2 M1 and V2 = VCM = , = − VCM = M1 + M2 M1 + M2

where η =

so that the asymptotic value of the angular momentum is given by: M1 1 b1 + M2 2 b2 =

M1 M2 (b1 + b2 ) = μ b . M1 + M2

(1.64)

The angular momentum at any point is given by: 2 2 M2 M1 2 ˙ 2 ˙ M1 r1 ψ + M2 r2 ψ = M1 r + M2 r ψ˙ M1 + M2 M1 + M2 = μ r2 ψ˙ ,

(1.65)

hence:

μ r2 ψ˙ = μ b .

(1.66)

Substituting from Eq. (1.66) into Eq. (1.63) to eliminate ψ˙ and solving for r˙, we obtain: r˙ =

1/2

1/2 2 b2 η Ei 1 − 2 − V (r) . μ r

(1.67)

The algebra for this step is as follows. Multiplying out the terms of Eq. (1.63) gives: 1 1 2 b 2 η Ei − μ r˙2 = μ 2 + V (r) , 2 2 r and re-arranging gives: 1 2 b 2 1 η Ei − μ 2 = μ r˙2 + V (r) . 2 r 2

(1.68)

28

1 The Radiation Damage Event

Recall that Ei = 1/2M12 and therefore, 2 = 2Ei /M1 and we can eliminate so μ b 2 Ei that the second term on the left hand side of Eq. (1.68) becomes − . Since M1 r2 M1 M2 μ= and μ /M1 = η , then: M1 + M2 b2 μ r˙2 μ r˙2 b2 + V (r) , and η Ei 1 − 2 = + V (r) , η Ei − η Ei 2 = r 2 r 2 or r˙ =

1/2

1/2 2 b2 η Ei 1 − 2 − V (r) , μ r

which is the same as in Eq. (1.67). Note that r reaches the distance of closest approach when r˙ = 0. At this point: b2 V (r) = η Ei 1 − 2 , r

(1.69)

and Vmax = η Ei (at b = 0) which represents a “head-on” collision. So if a particle strikes a target atom of equal mass, then V max = 1/2Ei . 2 2 When r → ∞, V (r) → 0 and r˙ = η Ei , or r˙2 = 2Ei /M1 , Ei = 1/2M1r˙2 (and μ r˙ = at r → ∞), so Ei = 1/2M1 2 . Recall that we are looking for φ as a function of b. Going back to Eq. (1.67) and dividing r˙ in Eq. (1.67) by ψ˙ from Eq. (1.66) we have: 1/2

1/2 2 2 r dr r˙ b2 . = =− μ Ei 1 − 2 − V (r) ψ˙ dψ μ r b

(1.70)

The minus sign in front of the quantity to the right of the equality is because for the first half of the orbit, r˙ decreases as ψ increases. Bringing the term r2 under the square root gives: 1 dr =− dψ b

1/2 1/2 2 μ Ei r4 − r2 b2 − r4V (r) . μ

(1.71)

Dividing terms under the square root by η Ei b2 to bring this term out of the square root gives: dr 1 =− dψ b

4 1/2 1/2 r 2 V (r) (η Ei )1/2 b 2 1 − . − r2 μ b η Ei

(1.72)

1.2 Interactions Between Ions and Atoms

Since 1/2M1 2 = Ei , then = (2Ei /M1 )1/2 , and substituting for gives: 1/2 4 1/2 2 M1 dr r V (r) 2 =− η Ei 1 − − r dψ μ 2Ei b2 η Ei 1/2 4 1/2 M1 r V (r) 2 η =− 1 − − r μ b2 η Ei

4 1/2 r V (r) = − 2 1− . − r2 b η Ei

29

(1.73)

Substituting for x = 1/r gives:

1/2 1 dx V (x) 2 = 2 1− . −x dψ b η Ei

(1.74)

This is the equation of orbit (ψ = f (x)). The scattering angle φ is found by expressing dψ as a function of x and dx and integrating from the limits on ψ corresponding to x = 0 and 1/ρ . These limits are φ /2 and π /2, respectively, as shown in Fig. 1.10. Performing this integration for the first half of the orbit yields: π /2 φ /2

dψ =

1/ρ 1 0

1−

b2

−1/2 V (x) dx − x2 η Ei

(1.75)

and

φ = π −2

1/ρ 1 0

b2

1−

−1/2 V (x) dx . − x2 η Ei

(1.76)

The quantity ρ in the upper limit of x is the value of r when ψ = π /2 and hence is the distance of closest approach, Since dx/ dψ = 0 when ψ = π /2, ρ is given from Eq. (1.74) by:

η Ei =

V (ρ ) . b2 1− 2 ρ

(1.77)

Equations (1.76) and (1.77) provide the relation between φ and b. We have yet to determine the cross section for our scattering event. This may be done as follows. If particles M1 are bombarding target atoms M2 , then in Fig. 1.11, those ions which cross an area 2π b db enclosed by circles of radii b and b + db will be scattered into dφ about φ . Since the relation between db and dφ can be obtained from Eq. (1.76) by differentiation, the differential cross section is

30

1 The Radiation Damage Event

Fig. 1.11. Scattering of ions crossing an area 2π b db into an angular element dφ about φ

given by:

σ (Ei , T ) dT = 2π b db and σ (Ei , T ) = 2π b

db dφ . dφ dT

(1.78)

Knowing V (r) enables φ to be written in terms of b2 using Eq. (1.76) and then in terms of T using Eq. (1.13). Differentiating gives 2π b db as a function of T and dT . Then from Eq. (1.78) the differential cross section for collisions having recoils in dT about T follows. The total cross section for collisions with T anywhere in the range Tˇ to γ Ei is:

σ (Ei ) =

γ Ei Tˇ

σ (Ei , T ) dT .

(1.79)

The process for finding the energy transfer cross section can be summarized as follows: 1. 2. 3. 4.

Select a potential function V (r). Use Eq. (1.76) to obtain b as a function of φ , b = f (φ ). Use Eq. (1.13) to obtain φ as a function of T , φ = g(T ). Use the relations between b and φ and between φ and T in Eq. (1.78) to obtain the energy transfer cross section.

The preceding description of the energy transfer cross section emphasizes the importance of knowing the potential function describing the particular ion–atom or atom–atom interaction of interest. Without accurate knowledge of the potential function, further description of the collision process and the ensuing defect structure become impossible. Unfortunately, explicit evaluation of the integral in Eq. (1.76) is possible only for simple potential functions. But before looking further at the various potential functions and their application in determining the energy transfer cross section, we need first to consider the different possible classes of ions and their corresponding energies.

1.2 Interactions Between Ions and Atoms

31

Classification of Ions There are three important classes of ions in ion–atom collisions. The first is light energetic ions with Ei > 1 MeV. The second is highly energetic (Ei ∼ 102 MeV) heavy ions such as fission fragments (M ∼ 102 ). The third is lower energy heavy ions that may be produced by an accelerator or appear as a recoil that result from an earlier high-energy collision. The energy of these recoils is generally less than 1 MeV. For each of these interactions, we must decide on the most appropriate potential function. A convenient guide is ρ /a, the ratio of the distance of closest approach to the screening radius as a function of the recoil energy, T . A rough graph of ρ vs. T is provided in Fig 1.12 to aid in the selection of the most appropriate potential. The three curves represent ions of each of the three classes just discussed: (1) 20 MeV protons, (2) 70 MeV fission fragments, and (3) 50 keV Cu ions. Curve (1) collisions apply to the regime where ρ a and the simple Coulomb potential is adequate. Curve (2) collisions that are head-on will have ρ a also. But for glancing collisions, ρ ∼ a and the screened Coulomb potential is most appropriate. Curve (3) represents the region where a < ρ 5a and the inverse square potential or Brinkman potential would apply since both the Born–Mayer and screened Coulomb terms must be accounted for.

Fig. 1.12. Distance of closest approach r, as a function of T for (1) 20 MeV protons in Cu, (2) 70 MeV Xe+ ions in Cu, and (3) 50 keV Cu+ recoils in Cu (from [12])

32

1 The Radiation Damage Event

Hard-sphere Type Collisions The hard-sphere potential is appropriate for ion energies below about 50 keV and for near head-on elastic collisions. Here, ρ ∼ re and atoms will act like hard spheres. In a head-on collision, b = 0 and from Eq. (1.77) we have:

η Ei = V (ρ ) .

(1.80)

When b is not quite zero, the collision may be pictured as in Fig. 1.13 where we M2 M1 define R1 = ρ and R2 = ρ . If ρ is known, then from the figure: M1 + M2 M1 + M2 b = ρ cos

φ . 2

(1.81)

Now, recalling that:

σs (Ei , T ) dT = 2π b db db dφ , σs (Ei , T ) = 2π b dφ dT

(1.82)

2 db dφ = = 1/2ρ sin φ /2 from b = ρ cos φ /2, and from dφ dT γ Ei sin φ γ Ei ρ 2 (1 − cos φ ). Then σ (Ei , T ) = 2πρ cos φ /2 sin φ /2 , and T= 2 2 γ Ei sin φ

where

σs (Ei , T ) =

πρ 2 . γ Ei

(1.83)

Fig. 1.13. Schematic of colliding atoms obeying the hard-sphere approximation for collisions

1.2 Interactions Between Ions and Atoms

33

Recall that for neutron–nuclear interactions, σs (Ei , T ) = σs (Ei )/γ Ei . Using this relation, we can obtain an idea of the size of the energy transfer cross section σ (Ei , T )a−a = for neutron–nuclear interactions vs. atom–atom interactions: σ (Ei , T )n−nuclear πρ 2 π (10−8 )2 ∼ ∼ 108 , and so the energy transfer cross section for atom–atom σs (Ei ) 10−24 interactions is about eight orders of magnitude greater than that for neutron–nuclear interactions. The total scattering cross section is:

σs (Ei ) =

γ Ei Tˇ

σs (Ei , T ) dT =

γ Ei πρ 2 Tˇ

γ Ei

dT =

πρ 2 γ Ei − Tˇ = πρ 2 . γ Ei

(1.84)

Note that σs (Ei ) is independent of Ei (because ρ = f (Ei )), and that σs (Ei , T )α 1/Ei and is independent of T . We can find σs (Ei , T ) explicitly by applying the appropriate potential function to find a value of ρ (determined by V (r)). Recall from our discussions in Sect. 1.2.1 that for collisions in which the impact parameter is on the order of the equilibrium separation of the atoms, the Born–Mayer potential is most appropriate. This corresponds to energies below about 10 keV. (Note that this means that we are also backing off from a pure hard-sphere model.) Hence, we will use V (r) = A exp(−r/B), where A and B are defined in Eq. (1.47). Using Eq. (1.80) gives: V (ρ ) = A exp(−ρ /B) = η Ei or

ρ = B ln

A η Ei

(1.85)

,

(1.86)

and since b = ρ cos φ /2 = B ln(A/η Ei ) cos φ /2, the energy transfer cross section is:

σs (Ei , T ) =

π B2 A 2 . ln γ Ei η Ei

(1.87)

The total scattering cross section is then the integral of the energy transfer cross section between the limits Tˇ and γ Ei :

σs (Ei ) =

γ Ei Tˇ

A 2 1 π B2 ln dT . η Ei γ Ei

(1.88)

From this expression, we will be able to calculate the total cross section for displacement scattering events for all allowed T . Note that the total scattering cross section depends on Ei . Also, for typical values of A, B and Tˇ (25 eV), the value of σs (Ei ) for atom–atom interactions is about 108 times that for neutron–nuclear events.

34

1 The Radiation Damage Event

Rutherford Scattering Let us turn now to a second example in which we will use the pure Coulomb scattering potential to demonstrate Rutherford scattering. From our classification of ions according to ion energy and mass, type 1 collisions involve light (m ∼ 1 to 4) energetic (E > MeV) ions where ρ a. Collisions of this sort are adequately represented by the simple Coulomb potential, which from Eq. (1.48) is: V (r) =

Z1 Z2 ε 2 . r

We will assume that Z1 and Z2 represent the nuclear charges and that this collision occurs at high energies so that electrons are stripped from the nuclei and the only interaction is between the nuclei. In our description of the trajectories of the particles in the CM system, we found that at the point of closest approach, dx/ dψ = 0 and from Eq. (1.77):

η Ei =

V (ρ ) . b2 1− 2 ρ

Substituting in for V (r) gives: Z1 Z2 ε 2 b2 = η Ei 1 − 2 . ρ ρ Defining: Z1 Z2 ε 2 , b0 = η Ei

(1.89)

(1.90)

it follows that: b0 b2 = 1− 2 , ρ ρ

(1.91)

and

ρ=

1/2 4b2 b0 1+ 1+ 2 . 2 b0

(1.92)

Hence, the distance of closest approach is a function of the impact parameter b, as expected. For head-on collisions, b = 0 and the minimum value of ρ depends on Ei :

ρ (b = 0) = ρ0 = b0 =

Z1 Z2 ε 2 . η Ei

(1.93)

1.2 Interactions Between Ions and Atoms

35

Note that for this type of collision, ρ depends on Ei , in contrast to independence of Ei in the hard-sphere model. Going back to the orbital equation (1.75), we will now evaluate it as a definite integral: φ /2 π /2

dψ =

0

1

b2

1/ρ

−

b0 x − x2 b2

−1/2

dx .

(1.94)

Since ψ = π /2 when r = ρ (x = 1/ρ ) and ψ = φ /2 when r = ∞ (x = 0), letting b0 y = x + 2 , gives: 2b

φ /2 − π /2 = where

c2

=

b0 2b2 b0 1 ρ + 2b2

c2 − y2

−1/2

dy ,

(1.95)

b20 1 + . The orbits are then: b2 4b4

b y 02 φ /2 − π /2 = sin−1 2b c ρ1 + 2bb02

b0 b0 1 −1 1 . = sin − sin + 2b2 c ρ 2b2 1 b0 −1 1 + Since sin = sin−1 (1) = π /2, then: c ρ 2b2 −1

sin φ /2 =

b0 . 2b2 c

(1.96)

(1.97)

Substituting for c (from above) into Eq. (1.97) yields: sin2 φ /2 =

1 . 4b2 1+ 2 b0

(1.98)

Using trigonometric relations for sin2 φ /2, we have: b=

b0 cot φ /2 . 2

(1.99)

We now have a relationship between the impact parameter, b and the asymptotic scattering angle, φ . Note that b is a function of Ei through b0 (Eq. (1.93)).

36

1 The Radiation Damage Event

We now want an expression for the scattering cross section. Using Eq. (1.82) for σs (Ei , T ), we have:

σs (Ei , T ) dT = σs (Ei , φ ) dΩ = 2π b db = π b0 cot

φ db , 2

(1.100)

and substituting for db from Eq. (1.99) gives:

σs (Ei , φ ) =

b0 4

2

1 , sin (φ /2)

(1.101)

4

which is the Rutherford inverse fourth power scattering law. The cross section for recoil is exactly the same as for elastic collisions, Eq. (1.13), and since:

σs (Ei , T ) = σs (Ei , φ )

dΩ , dT

we have:

σs (Ei , T ) =

π b20 Ei γ . 4 T2

(1.102)

Note that unlike neutron–nuclear collisions and hard-sphere scattering in general, the Rutherford scattering cross section is a strong function of T . This expression also shows that the scattering cross section σs (Ei , T ) → ∞ as T → 0. But this is just a reflection of the fact that as φ → 0, b → ∞ and is representative of longrange Coulomb interactions. In reality, there is a cut-off in b and hence in φ due to electron screening. As we will see later, this cut-off is Ed , the displacement energy. The average energy transferred is then: Tˆ

Tˇ ln(Tˆ /Tˇ ) ˇ T σs (Ei , T ) dT T¯ = T ˆ . = T Tˇ Tˇ σs (Ei , T ) dT 1− Tˆ For Tˆ = γ Ei and Tˇ = Ed and since γ Ei Ed , then: γ Ei T¯ ≈ Ed ln . Ed

(1.103)

(1.104)

which is quite small for all energies Ei , reflecting the strong 1/T 2 dependence in Eq. (1.102). The integral of Eq. (1.102) over T gives the total cross section for displacement events by an ion of energy Ei :

π σs (Ei ) = b20 Tˆ 4

Tˆ dT Ed

π b20 = T2 4

Tˆ −1 , Ed

(1.105)

1.2 Interactions Between Ions and Atoms

37

and since at high energies Tˆ /Ed 1 then we have for Tˆ = γ Ei :

σs (Ei ) ≈

π b20 γ Ei , 4 Ed

(1.106)

which is quite large. A critical question in applying the above results is under what conditions can Rutherford scattering be applied? The answer is that we must require that during an encounter, the major part of scattering occurs in the region where r a. But this is a qualitative measure. What is needed is a means for determining quantitatively, when Rutherford scattering applies. To address this question, we consider two cases. Case 1: Near “head-on” collisions high T . For near head-on collision, ρ0 a or Ei Ea , where Ea is the value of Ei that would give ρ0 = a assuming a screened Coulomb potential: Ea = 2ER (Z1 Z2 )7/6 (M1 + M2 ) /(M2 e) ,

(1.107)

which is obtained by re-writing the screened Coulomb potential (Eq. (1.49)) in an inverse square law form (Eq. (1.59)), with ε 2 = 2a0 ER and equating at r = a and M2 setting V (r) = η Ei = Ei for a head-on collision. M1 + M2 Case 2: Glancing collisions (low T). Here we only consider those collisions in which b ≤ a, or that result in an energy transfer Tˇ ∼ Ed for b = a. For a simple Coulomb collision with b = a, we have from Eqs. (1.98) and (1.13): T=

ε 2 γ Ea2 , 4Ei

or Ei =

ε 2 γ Ea2 , 4T

(1.108)

and giving this value of Ei the name Eb at T = Tˇ , we have Eb =

ε 2 γ Ea2 , 4Tˇ

where Tˇ = Ed ,

(1.109)

and this equation is valid for all Ei Eb . Essentially, Eb is the value of Ei that results in a transfer of energy T ≥ Ed at b = a. Or looking at it another way, values of Eb < Ei give T Tˇ and can be neglected since ρ ≥ a, and these encounters can be neglected. Table 1.4 provides examples of the values of Ea and Eb for different particle–target atom combinations and energies. From Table 1.4, since Ea < Eb , we can use the criterion that Ei must be Eb as an extreme test of the validity of the simple Coulomb scattering description. In summary, if Ei Ea , the simple Coulomb potential may be used for near head-on collisions. If Ei Eb , it can be used for all collisions of interest in radiation damage. Light charged particles such as protons and alphas with Ei > 1 MeV fall into this category, while fission fragments are in the regime Ea < Ei < Eb and recoils have Ei ≤ Ea . These will be discussed next. But first, we present an example of Rutherford scattering.

38

1 The Radiation Damage Event

Table 1.4. Values of Ea and Eb for various particle–target atom combinations and energies (from [13]) Incident particle C Al Cu Au Xe D+ D+ D+

Target atom

Ea (eV) 2 × 103

C Al Cu Au U C Cu U

1 × 104

7 × 104 7 × 105 5 × 105 1.5 × 102 1 × 103 4 × 103

Eb (eV) 8 × 105 2 × 107 1 × 109 1 × 1011 3 × 1010 2 × 103 2 × 104 1 × 105

Example 1.2. 2 MeV protons on aluminum For this case, Tˆ = γ Ei =

4(27) 2 MeV = 0.28 MeV (27 + 1)2

Tˇ = 25 eV

γ Ei T¯ = Ed ln Ed

= 233 eV

We can also calculate Ea ∼ 200 eV and Eb ∼ 4000 eV. (For comparison, 2 MeV He+ on Al, Ea ∼ 1 keV and Eb ∼ 25 keV. Also, for 2 MeV H+ on Au, Ea ∼ 1.6 keV and Eb ∼ 38 keV, and for 2 MeV He+ on Au, Ea ∼ 8 keV and Eb ∼ 69 keV.) Since Ei Eb , the simple Coulomb law is valid for this type of collision. Incidentally, σ (Ei ) ∼ 4 × 10−22 cm2 and since the mean free path between collisions is λ = 1/σ N and N ∼ 6 × 1022 a/cm3 , then λ ∼ 0.04 cm or about 400 μm, or about 10 times the length of a 2 MeV proton track in Al. This means that there is on average, only one Rutherford scattering collision for every 10 protons incident on Al.

Now, lets investigate the other classes of ion–atom collisions such as heavy, energetic ions, heavy, slow ions and high-energy electrons. Heavy, Energetic Ions For heavy, energetic ions such as fission fragments, Fig. 1.12 shows that an appropriate potential must account for both screened Coulomb and closed shell repulsion. Let us look first at the simple Coulomb potential as a rough approximation, knowing that its use is only justified for recoil energies approaching γ Ei which is where

1.2 Interactions Between Ions and Atoms

39

π b20 γ Ei 4M1 M2 M2 Z1 , and b0 α ,γ= ,η= , 2 4 Ed γ Ei M (M1 + M2 ) 1 + M2 which gives an increase in the cross section compared to the light ion by a factor of z21 M1 Ei heavy σheavy = 2 ≈ 106 σlight z1 M1 Ei

ρ a. Recall that σ (Ei ) =

light

light

for the fission fragments at the peaks of the fission yield of uranium, M1 96 amu, light heavy heavy E1 95 MeV and M1 137 amu, E1 55 MeV. Comparing to the example of the 2 MeV proton on Al, fission fragments have a cross section that is larger by a factor of 104 ! Therefore, the mean free path is 10−4 that of a proton in Al. Recall that σ (Ei , T ) varies as 1/T 2 . But this is only true near γ Ei (ρ a). At lower energies screening will reduce the sensitivity to energy. So we must use a better description of the interaction between energetic, heavy ions and target atoms. Brinkman’s expression, Eq. (1.50), includes both terms and if this is used in the impulse approximation (see [13]), the result is:

b b 2 M1 A2 , T= F α, − (1 − α ) F 1 + α , M2 Ei B B where A, B are given in Eq. (1.50) and − e−x dx b b ∞ = F α, B B b/a (x2 − b2/a2 )1/2 (1 − e−α x )2 b b ∞ (1 + nα ) , = ∑ (n + 1) K0 B n=0 B

(1.110)

(1.111)

where K0 (y) is a Bessel function of the third kind. The term α is the ratio of Born– Mayer and screened Coulomb terms at r = a, so in general, α < 1. T can be found from b and Eq. (1.110), and by inversion, b is obtained as a function of T . Differentiation gives σ = 2π b db. However, because of the complexity of Eq. (1.110), numerical solutions are required. Nevertheless, we may calculate dN, the number of recoils in dT at T produced by the fission fragment in slowing down to rest. This is found by: dσ dN = nσ dx = n dT

dE − dx

−1

dE dT ,

(1.112)

40

1 The Radiation Damage Event

Fig. 1.14. The energy spectrum of recoils N(T ) dT produced by fission fragments slowing down to rest in uranium. Two cases are shown: M1 = 96, E1 = 95 MeV and M1 = 137, E1 = 55 MeV (from [13])

where n is the density of atoms, and N (T ) dT = n

Ei σ dE −1 0

dT

dX

dE dT .

(1.113)

Brinkman carried out these calculations for light and heavy fragments from 235 U fission slowing down in uranium. The results are shown in Fig. 1.14. Note that N(T ) decreases more rapidly than T −1 and hence the majority of displaced atoms are produced by low-energy recoils. Therefore, high-energy recoils can be neglected altogether. Another way of looking at this is that the simple Coulomb potential is only valid in an energy range that does not contribute significantly to displacements. Heavy, Slow Ions These ions are classified by the curve labeled “3” in Fig. 1.12. This is a very important class of collisions as it covers most of the applications of kV ion implanters and low MeVaccelerators in the fields of materials science and radiation damage that includes such topics as ion implantation and heavy ion radiation effects simulation. The figure shows that collisions must be dealt with over the range a < ρ < 10a. The formalism used for fission fragments in the previous section applies to glancing collisions but for head-on collisions, another approach is needed. The appropriate

1.2 Interactions Between Ions and Atoms

41

potential for a/5 ≤ ρ ≤ 5a is the inverse square approximation. We use a potential of the form: a 2 2ER 0 (Z1 Z2 )5/6 , V (r) = e r which is obtained by fitting a screened Coulomb potential to the inverse square potential and equating at r = a, Eq. (1.59). Substituting this potential function into the orbital equation (1.76) gives: −1/2 φ a 2 Ea = 1− 1+ 2 . π b Ei

(1.114)

Using Eq. (1.13) to express φ in terms of T gives: −1/2 a 2 Ea 2 π T = γ Ei cos . 1+ 2 2 b Ei

(1.115)

Expressing b in terms of T and differentiating gives:

σs (Ei , T ) =

4Ea a2 α

γ Ei2 (1 − 4α 2)2 [x (1 − x)]1/2

,

(1.116)

T and πα = cos−1 x1/2 . γ Ei For small x (low-energy transfer), we have:

where x =

σs (Ei , T ) =

π 2 a2 Ea γ 1/2 1/2 3/2

8Ei

T

.

(1.117)

Note that the energy transfer cross section is dependent on T . The mean recoil energy is: γ Ei

1/2 ˇ T σs (Ei , T ) dT T¯ = T γ E = γ Ei Tˇ . i σ (E , T ) dT s i ˇ T

(1.118)

The total cross section for displacement is:

σs (Ei ) =

γ Ei Tˇ

π 2 a2 Ea γ 1/2 σs (Ei , T ) dT = 1/2 . 4 Ei Tˇ

(1.119)

Relativistic Electrons Radiation damage from electrons is not so important in reactor core materials, but more so in the laboratory as they are commonly used in electron microscopes for radiation damage studies. Due to the low mass of the electron, very high energies

42

1 The Radiation Damage Event

must be attained in order to cause displacements of a lattice atom. These energies are high enough such that relativistic quantum mechanics must be used to describe the collision. Even so, the energy transferred is large enough to displace only the struck atoms with no secondary displacements. In relativistic form, the momentum of an electron with rest mass m0 and kinetic energy Ei is: p2e =

Ei Ei + 2m0c2 . 2 c

(1.120)

Since the struck atom recoils non-relativistically, the recoil expression is that given in Eq. (1.9): 2 2 2 V2 = VCM + Vc2 − 2VCMVc cos φ = 2VCM (1 − cos φ ) = 4VCM sin2

φ , 2

and conservation of momentum gives: pe = (m0 + M) VCM ∼ = MVCM . Replacing the velocity terms with energies in the expression for V2 yields: T=

φ 2Ei Ei + 2m0c2 sin2 , 2 Mc 2

(1.121)

or 2Ei Tˆ = Ei + 2m0c2 . 2 Mc

(1.122)

An approximate expression for the Dirac equation for light ions [13] yields the differential scattering cross section:

σs (E1 , φ ) =

4π a20 Z22 ER2 1 − β 2 β4 m20 c4 2 2 × 1 − β sin (φ /2) + παβ sin (φ /2) (1 − sin (φ /2)) × cos (φ /2) csc3 (φ /2) ,

(1.123)

where β = v/c and α = Z2 /137. This expression approaches the Rutherford scattering law for small β . Using Eqs. (1.121) and (1.122), the differential scattering cross section is written in terms of T and Tˆ : 4π a20Z22 ER2 1 − β 2 T 1/2 T α Tˆ 2T σs (Ei , T ) = − . 1−β +π 2 4 4 β β T2 m0 c Tˆ Tˆ Tˆ (1.124)

1.2 Interactions Between Ions and Atoms

The total cross section is found by integrating Eq. (1.124) from Tˇ to Tˆ : 4π a20Z22 ER2 1 − β 2 Tˆ Tˆ 2 σs (Ei ) = β log − 1 − 2 4 β m0 c 4 Tˇ Tˇ 1/2 Tˆ Tˆ − 1 − log . +αβ 2 Tˇ Tˇ

43

(1.125)

For electrons with energies above the damage threshold and Tˆ /Tˇ slightly greater than unity:

σs (Ei ) ∼ =

4π a20Z22 ER2 m20 c4

1−β2 β4

2

Tˆ −1 . Tˇ

(1.126)

Figure 1.15 shows that at high enough energies, σ (Ei ) approaches an asymptotic value:

σs (Ei ) →

8π a20 Z22 ER2 Tˇ M2 c2

(1.127)

when Ei m0 c2 . It should be emphasized, however, that these cross sections are most accurate for light elements but seriously underestimate σs (Ei ) for heavy elements (Z > 50). Table 1.5 provides a summary of the energy transfer and the energy transfer cross sections for the various types of atom–atom interactions discussed in Sect. 1.2.

Fig. 1.15. Damage cross section for electrons bombarding copper where Ed = 25 eV (from [13])

44

1 The Radiation Damage Event

Table 1.5. Energy transfer and energy transfer cross sections for various types of atom–atom collisions Type of collision

Hard-sphere type (Born–Mayer potential) ρ ∼ re Rutherford scattering (simple Coulomb potential) ρ a Heavy ion (inverse square) a/5 ≤ ρ ≤ 5a Relativistic electrons

Energy transfer and energy transfer cross section

π B2 A 2 σs (Ei , T ) = ln γ Ei η Ei ¯ T = γ Ei /2

π b2 E γ σs (Ei , T ) = 0 i2 4 T γ E i T¯ ≈ Ed ln Ed σs (Ei , T ) =

π 2 a2 Ea γ 1/2 1/2 3/2

8Ei

Equation in text (1.87) (1.13) (1.102) (1.104) (1.117)

T

1/2 T¯ = γ Ei Tˇ 4π a20 Z22 ER2 1 − β 2 σ (Ei , T ) = β4 m20 c4 T 1/2 T T α Tˆ 2 +π × 1−β − 2 ˆ ˆ ˆ β T T T T

(1.118)

(1.124)

1.3 Ionization Collisions Up to this point, we have been treating collisions as discrete events. However, besides collision with or between nuclei, an ion or atom traveling through the lattice may lose energy by electronic excitation, by ionization or by Bremsstrahlung (loss of energy of an electron passing through the Coulomb field of a nucleus by emission of X-rays). These events may be viewed as more or less continuous events. What follows is a treatment of energy loss in solids. 1.3.1 Energy Loss Theory We are interested in finding the differential energy loss of an ion or atom traveling through a lattice. We begin by defining the energy loss per unit length as − dE/ dx (or NS(E) where N is the atom number density and S is the stopping power in units of energy × distance squared) so that the total energy loss can then be approximated by a sum of these components: dE dE dE dE = − + − + − , (1.128) − dx total dx n dx e dx r

1.3 Ionization Collisions

45

where the subscripts are defined as follows: n = elastic e = electronic r = radiation For most of the applications in which we will be interested, energy loss by radiation will be small and will be neglected. From our discussion in Sect. 1.2.1 it is evident that in order to accurately describe the slowing down of an ion or atom over the entire energy range from Tˆ to Tˇ , where Tˆ may be in MeVand Tˇ ∼ 10 eV, several potential functions would need to be “pieced” together (see Fig. 1.9). This would cause problems because of discontinuities at the cuts. Moreover, the cut-off points of these functions often differ depending on M and Z. However, we can separate or subdivide stopping power according to the type of interaction and hence, the energy regime. In the high-energy regime, ρ a and Se Sn and these interactions are treated as pure Coulomb collisions. In the lowenergy regime, ρ ≈ a and Sn > Se . This is the region of importance in the deposition of displacement energy. In either case, we can establish a formalism for calculating stopping power, dE/ dx = NS(E). If we know the energy transfer cross section σ (Ei , T ) for either Sn or Se , then we can calculate the average energy transfer:

T σ dT = energy lost or transferred, T¯ = σ dT 1 and the mean free path (mfp) between collisions is λ = σ . Then the ratio of these N two quantities is the energy loss per unit length:

Tˆ Tˆ dE T¯ ˇ T σ (Ei , T ) dT = = T ˆ σ (Ei , T ) dT ·N T dx λ Tˇ Tˇ σ (Ei , T ) dT

=N

Tˆ Tˇ

T σ (Ei , T ) dT ,

(1.129)

where N is the target number density. Another way to look at this is as follows: Consider a projectile incident on an amorphous target containing an average of N atoms/unit volume (Fig. 1.16). In traversing the slab of material between x and x + Δx, the projectile will come within a distance b1 of NΔx2π b1 db target particles and transfer an energy T (Ei , b) to each. The total energy transferred to all target particles in the slab is obtained by integrating over all possible impact parameters: ΔE = NΔx

∞ 0

T 2π b db.

46

1 The Radiation Damage Event Fig. 1.16. Schematic of an incident projectile of energy E passing within a distance b1 of an annular ring containing NΔx2π b1 db atoms

Assuming ΔE E and dividing by Δx and taking the limit as x → 0, we obtain: ∞ ΔE dE = N = T 2π b db. Δx lim x→0 dx 0 We know that σ (Ei , T ) dT = 2π b db, so: dE =N dx

Tˆ Tˇ

T σ (Ei , T ) dT ,

which is the same result as from Eq. (1.129). Let us first consider nuclear stopping, or energy loss from elastic collisions. Nuclear Stopping Power dE We define − or NSn (Ei ) as the energy lost to target nuclei when a projectile dx n of energy Ei traverses adifferential thickness dx of a target of unit density. A simple dE can be made if we assume that each target nucleus acts formulation of − dx n independently of every other target nucleus in slowing down a projectile. In essence, we are neglecting any possible interactions between nuclei. This is a fair approximation for amorphous targets and a good first approximation for crystalline targets also. Case 1: High-energy Elastic Collisions, ρ a. Rutherford scattering describes this type of interaction accurately. Recall that for simple Coulomb scattering, the energy transfer cross section (Eq. (1.102)) is:

σs (Ei , T ) =

π b20 γ Ei . 4 T2

1.3 Ionization Collisions

Therefore the stopping power becomes: γ Ei π b2 γ E dE = NS (E ) = N T 0 2i dT n i dx n 4 T Tˇ 2 N π b0 γ Ei = γ Ei ln , 4 Tˇ

47

(1.130)

ε 2 γ Ea2 where Tˆ = γ Ei and Tˇ is the value of T which yields b = a or Tˇb = . 4Ei Substituting for b0 from Eq. (1.93) gives: dE γ Ei N π Z12 Z22 ε 4 M1 = NS (E ) = ln . n i dx n Ei M2 Tˇb

(1.131)

Note that for like atoms, γ = 1 and M1 = M2 , so: NSn (Ei ) =

N π Z12 Z22 ε 4 Ei ln . Ei Tˇb

(1.132)

Substituting for Ea from Eq. (1.107) into the expression for Tˇb gives: 4E 2 (Z Z )2 (Z1 Z2 )2/6 Tˇb = R 1 2 . Ei

(1.133)

Using a = a0 /(z1 z2 )1/6 and substituting for (z1 z2 )1/6 gives: 4E 2 a2 Z 4 Tˇb = R2 0 , a Ei for z1 = z2 , and since ε 2 = 2a0 ER , then Eq. (1.132) becomes: 4N π Z 4 a20 ER2 Ei ln NSn (Ei ) = Ei Tˇb 2 2 4N π Z 4 a20 ER2 a Ei = ln Ei 4a20 ER2 Z 4

(1.134)

Case 2: Low-energy elastic collisions, ρ ∼ a. At intermediate and lower energies, pure Coulomb scattering will not correctly capture the interaction. Here we must use a screened Coulomb function to account for the effects of the electrons in the internuclear space. Lindhard, Nielsen and Scharff [14] proposed a universal, one-parameter, differential scattering cross section in reduced notation: −π a2 f t 1/2 σ= (1.135) 2 t 3/2

48

1 The Radiation Damage Event

where t is a dimensionless collision parameter defined by: t =∈2

T , Tˆ

(1.136)

and ∈ is dimensionless energy defined as: ∈=

aM2 Ei . Z1 Z2 ε 2 (M1 + M2 )

(1.137)

Lindhard et al. [14] treated f t 1/2 to be a simple scaling function where t was a measure of the depth of penetration into an atom during a collision and large t represents close approach. The function f t 1/2 is plotted as the thick solid line in Fig. 1.17. The analytical expression for the function developed by Winterbon et al. [15] is: −3/2 , (1.138) f t 1/2 = λ t 1/6 1 + (2λ t 2/3 )2/3 where λ = 1.309. A generalization of Eq. (1.138) for power law scattering is: 1 −m 1/2 = λm t 2 , f t

(1.139)

where λ1/3 = 1.309, λ1/2 = 0.327, and λ1 = 0.5. Equation (1.139) approximately describes scattering from a potential of the form V (r)α r−s = r−1/m , where s is the

Fig. 1.17. Reduced differential cross section calculated from the Thomas–Fermi potential. The thick solid line ranging over 10−3 M2 , B = 1/3. Increased electronic stopping at higher energies leads to smaller values of B. When M1 < M2 , large angle scattering

Fig. 1.23. Reduced range-energy plots for various values of the electronic stopping parameter, k

62

1 The Radiation Damage Event

increases the difference between R and Rp . However, for these collisions, electronic stopping is appreciable and partially offsets the increase in the difference. Therefore, B = 1/3 is a reasonable approximation for a wide range of conditions, giving: Rp ∼ =

R . 1 + (M2/3M1 )

(1.199)

Range straggling can be calculated using the theory of Lindhard et al. [16]. For the case where nuclear stopping dominates and M1 > M2 , i.e., small angle scattering: 1/2 M ) 2(M 1 2 ∼ 1.1Rp 2.5ΔRp = , (1.200) M1 + M2 or ΔRp ∼ = Rp /2.5 .

(1.201)

For a high-energy ion, the slowing down path is essentially a straight line in the original direction of motion, since the stopping is electronic with a small amount of straggle at the end due to nuclear collisions (Fig. 1.24a). At lower energies where Sn

Fig. 1.24. Total path length, projected range and perpendicular range for (a) high-energy ions and (b) low-energy ions incident on a target

1.3 Ionization Collisions

63

and Se are more comparable, the ion path follows a zigzag course with many large deflections with the distance between collisions decreasing as the energy decreases and the cross section increases (Fig 1.24b). The stopping positions are distributed according to a Gaussian as N(x) = Np e−1/2X , 2

(1.202)

x − Rp and ΔRp is the standard deviation (Fig. 1.25). If the peak conΔRp 1 centration is Np at Rp , then this will fall to 1/2 Np at distances x = Rp ± ΔRp . If we e view the target perpendicularly through its surface, then the number of implanted ions per unit area will be Ns , given by:

where X =

Ns =

+∞ −∞

N(x) dx ,

(1.203)

or since dx = ΔRp dX and the Gaussian curve is symmetrical, then: Ns = 2ΔRp Np

∞ 0

e−1/2X dX , 2

which can be written: √ 2 ∞ −1/2X 2 Ns = ΔRp Np 2π e dX . π 0

(1.204)

(1.205)

Fig. 1.25. Parameters of the Gaussian distribution applied to an ion implantation profile showing the projected range, R¯ p , the straggling or standard deviation, ΔRp , and the maximum concentration, Np of the implanted ion

64

1 The Radiation Damage Event

The integral inside the bracket is the error function and tends to unity as X → ∞, so that if Ns is the number of ions/cm2 implanted into the target, we have: Ns 0.4Ns ∼ Np = √ , = ΔRp 2π ΔRp so the density of implanted ions is: x − Rp 2 0.4Ns . N(x) = exp −1/2 ΔRp ΔRp

(1.206)

(1.207)

As an example, if we implant 5 × 1015 ions/cm2 of 40 keV B into Si, then Rp ∼ 160 nm, ΔRp ∼ 54 nm and Np ∼ 4 × 1020 atoms/cm2 . Note that from the properties of the Gaussian, the concentration will fall by one decade at x Rp ± 2ΔRp and by 2 decades at x Rp ± 3ΔRp, etc. Using the LSS treatment to describe electronic and nuclear stopping, Littmark and Ziegler have solved for the ranges of atoms with atomic number between 1 and 92 in all elements. Their work is published in Volume 6 of The Stopping and Ranges of Ions in Matter [20]. For each atom serving as the target, the mean ion depth, longitudinal straggling and transverse straggling is compiled in graphs for projectiles with 1 ≤ Z ≤ 92 and over a wide energy range. The following example is taken from this handbook.

Example 1.3. MeV He implantation into Si Zeigler [18] plots and tabulates the range parameters for a wide range of ions and target atoms. For 2 MeV He incident on a Si target, the range and straggling are 7.32 μm and 0.215 μm, respectively. If we assume a dose of 1015 He ions/cm2, then applying Eq. (1.204) gives a peak concentration of ∼1.86 × 1019 He atoms/cm3 at a depth of 7.32 μm, which is approximately 620 appm. Equation (1.205) gives the distribution of deposited He atoms as: x − 7.32 2 19 He/cm3 , N(x) = 1.86 × 10 exp −1/2 0.215 where x is in units of μm.

In addition to a tabulation of range data, Ziegler has developed a Monte Carlo based computer program for calculating the transport of ions in matter [18]. The program is available on the web at http://www.srim.org and the reader is encouraged to try some examples using the SRIM simulation software. This program is downloadable at no cost to the user (subject to the terms of use posted on the site) and may be executed on your personal computer. The following example uses data taken from the SRIM program.

1.3 Ionization Collisions

65

Example 1.4. Implantation of Al into Ni A similar example can be worked for lower energy implantation of a heavier element such as Al, into a nickel target. In this case, we use the output of the TRIM program. Selecting 200 keV Al in Ni results in a projected range of ∼135 nm with a longitudinal straggling of 44 nm. Substitution into Eq. (1.204) yields a peak concentration 9.1 × 1019 Al/cm3 for a dose of 1015 Al+ /cm2 . The TRIM software also yields a quantity that allows the user to determine concentration. The unit of concentration in the ion range plot is [atoms/cm3/atoms cm2 ] and the range of the implanted ion distribution on this plot has a maximum of ∼8 × 104 atoms/cm3 /atoms cm2 . Multiplying this value by the dose of 1015 Al+ /cm2 gives ∼8 × 1019 Al/cm3 which is close to the analytical solution.

Chapter Review The chapter began with a description of neutron–nuclear collisions, utilizing the absence of charge on the neutron to describe the interaction using a hard-sphere approximation. Expressions for the energy transfer in elastic and inelastic scattering collisions were developed and (n, 2n) and (n, γ ) reactions were analyzed as well to determine the energy transferred. Table 1.2 summarizes the energy transfer and energy transfer cross sections for these types of reactions. The description of projectile-target interaction was broadened to include ion–atom and atom–atom collisions which are relevant for two important cases: ion irradiation or implantation and the interaction between atoms in a lattice after the initial collision with a neutron in reactor materials. Interatomic potentials form the basis for describing the interaction between atoms and also for determining the energy transfer cross section. Table 1.3 summarizes the important potentials used to describe these interactions. Collision kinematics was then used to develop a description of the orbit of colliding atoms and hence, the transferred energy and the energy transfer cross section. Because there is not one single interatomic potential that describes the interaction over the entire distance (energy) range, the energy transfer and energy transfer cross sections are analyzed in various energy ranges and for various classes of interactions. Rutherford scattering is used to describe light energetic ions and slow heavy ions, energetic heavy ions, and relativistic electrons are all treated separately. Table 1.5 summarizes the energy transfer and energy transfer cross section for various atom–atom collisions. Energy loss theory is developed in order to determine the energy loss of energetic atoms/ions to the solid by elastic/nuclear collisions and by collisions with the electrons of the target. Collisions are analyzed in terms of their energy range for both nuclear stopping and electronic stopping. Table 1.7 summarizes the stopping

66

1 The Radiation Damage Event

powers for various types of interactions. Finally, the stopping powers are used to develop expressions for the range and projected range of ions in solids so that their penetration depth and concentration distribution can be determined.

Nomenclature a a0 aU A A b B C c D Ea Eb Ed ED Ef Eγ Ei f Ev,i m Ev,i Em Em EM EM ER ET I¯ m M N Np Ns pe Q re r˙ R Reff

Screening radius Bohr radius of the hydrogen atom Universal screening length Atomic mass Pre-exponential constant in Born–Mayer relation, Eq. (1.47) Impact parameter Constant in exponent in Born–Mayer relation, Eq. (1.47) Constant in screened Coulomb potential, Eq. (1.49) = 0.8853 Speed of light Nearest neighbor spacing between atoms Value of Ei that yields ρ0 = a Value of Ei that gives T ≥ Ed at b = a Displacement energy Maxwellian nuclear temperature = kT Final energy Gamma ray energy Incoming particle energy Vacancy and interstitial formation energy Vacancy and interstitial migration energy Kinetic energy of incoming particle in CM system Energy of neutron after (n, 2n) reaction Kinetic energy of target particle in CM system Energy of CM after (n, 2n) reaction Rydberg energy Total energy Excitation-ionization level Mass of incoming particle Mass of target Atom number density Peak implanted ion concentration Implanted ion density in ions/unit area Momentum of electron Excitation energy of nucleus Nearest neighbor spacing between atoms Radial velocity in polar coordinates Range of ion Recombination radius

Nomenclature

Rp ΔRp s Se Sn t t T Tˇ Tˆ T¯ T V (r) c Vc c Vc c Vc VCM V V Z

Projected range Standard deviation of projected range Power law exponent Electronic stopping power Nuclear stopping power Time Dimensionless collision parameter, Eq. (1.136) Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy transferred to target atom after (n, 2n) reaction Potential energy Velocity of incoming particle in CM system Velocity of target particle in CM system Velocity of incoming particle in CM system after collision Velocity of target atom in CM system after collision Velocity of neutron in CM system after (n, 2n) reaction Velocity of target atom in CM system after (n, 2n) reaction Velocity of CM in lab system Velocity of incoming particle in lab system Velocity of incoming particle in lab system after collision Velocity of target atom in lab system after collision Velocity of target atom in lab system after (n, 2n) reaction Atomic number

β χ (r) χU ε ∈ φ φ ψ˙ ψ λ λm λ μ ν (T ) θ ρ ρe ρ0 ρr

/c Screening function Universal screening function Unit charge Dimensionless, reduced energy parameter, Eq. (1.137) Asymptotic scattering angle at infinity separation Scattering angle in CM system Angular velocity in polar coordinates Scattering angle of struck atom in lab system Mean free path between collisions See Eq. (1.139) 1.309, Eq. (1.138) Reduced mass, Eq. (1.63) Displacement function Scattering angle in lab system Distance between atom centers in a collision Electron cloud density Distance of closest approach; value of r when ψ = π /2 Dimensionless, reduced distance parameter, Eq. (1.141)

67

68

1 The Radiation Damage Event

σ (Ei ) σ (Ei , T ) σ (Ei , φ ) σ (Ei , Eφ , Ω ) σ (Ei , Q j , φ ) σ (Ei , Q j , T ) Ω dΩ ξe

Total atomic collision cross section Differential energy transfer cross section Differential angular collision cross section Double differential collision cross section Differential angular cross section for inelastic collisions Differential energy transfer cross section for inelastic collisions Solid angle into which incoming particle is scattered Differential solid angular element 1/6 Z1

Problems 1.1 A 0.5 MeV neutron strikes a target atom with mass A, which is initially at rest. Calculate the velocity and energy of both particles in the laboratory reference frame after a head-on collision for A = 27 (Al) and A = 207.2 (Pb). 1.2 A detector of 100% efficiency (i.e., every particle entering the detector is registered) and area of 1 cm2 is placed a distance r from a target (taken to be of zero dimension, i.e., a point). The target is bombarded with neutrons. Assuming that only elastic scattering occurs, that scattering is azimuthally symmetric and that the scattering cross section is isotropic: a) What is the ratio of the number of particles detected by the detector at positions 1 and 2 shown in the figure? b) What is the ratio of the number of particles scattered through an angular increment of 10◦ about θ1 = 5◦ and θ2 = 85◦ ? c) Repeat parts (a) and (b) assuming that instead of being isotropic, the differential scattering cross section varies as σs (Ei , θ ) = cos θ .

dθ = Increment of scattering angle dΩ = Increment of solid angle about θ θ = Scattering angle in the center-of-mass system

Problems

69

1.3 A Ti plate is bombarded with 1014 neutrons per cm2 per second at perpendicular incidence. The entire plate is hit by the beam. a) Calculate the number of particles scattered per second at i) 85◦ ≤ θ = 86◦ and ii) 5◦ ≤ θ = 6◦ . The plate size is 1 cm2 by 0.6 mm. Scattering is isotropic with a total scattering cross section of 2.87 barns (1 barn = 10−24 cm2 ). b) The same target is bombarded with particles such that the differential angular scattering cross section is proportional to θ 2 . Calculate the ratio of the atomic flux in interval (i) above to that in interval (ii). In both cases, perform full integration of the differential cross section. c) Approximate the integrals in (b) by assuming the differential angular scattering cross section to be constant in each integration interval and equal to the value at the interval’s center. 1.4 Derive the kinematic factor K, defined as K = Ef /Ei , where Ei is the projectile energy before the collision and Ef is the projectile energy after the collision. 1.5 The following formula relates the scattering angles θ and φ in the lab and center-of-mass frames, respectively: tan θ = (M/m) sin φ / [1 + (M/m) cos φ ]

1.6 1.7 1.8

1.9

where m and M are the masses of the projectile and target, respectively. Discuss this expression for the following three cases: m = M, m M and m M. Derive Eq. (1.24) in the text. Derive Eq. (1.39) in the text. For two colliding particles write expressions for: a) ET , the total energy of a system of n particles b) ECM , the energy of the center of mass (determined by VCM and the total mass of the system) c) and E, the total energy in the CM system. Show that E = ET − ECM (Eq. (1.61)) Derive a relation between b and φ from Eq. (1.76) for the hard-sphere potential: VHS (r) = 0 =∞

r ≥ r0 r < r0

Make sure your answer is correct for b > r0 . 1.10 As a means of describing atom–atom interaction at intermediate separation, i.e., between Coulombic repulsion and closed shell repulsion, an inverse power potential is often employed of the form V (r) = constant/rn . For example, one can fit an inverse square (n = 2) function to the screened Coulomb potential at r = a obtaining the same slope, ordinate and curvature.

70

1 The Radiation Damage Event

This function is

V (r) = z1 z2 ε 2 a/ r2 exp[1] .

1.11

1.12

1.13

1.14

1.15

1.16

1.17

1.18

1.19

Formulate the cross sections σs (Ei , T ) and σs (Ei , φ ) for atom–atom interactions obeying the inverse square potential function. Compare your result in Problem 1.10 to that obtained using a Born–Mayer potential and a simple Coulomb potential. Comment on the similarities and differences. Calculate the average energy transfer from a 100 keV Ni atom colliding with another Ni atom, using: a) The hard-sphere potential b) The inverse square potential. Explain, in physical terms, why the scattering cross section resulting from Coulombic repulsion depends on the transferred energy, T , while that for neutron–nuclear interaction does not. Assuming a pure Coulomb potential, determine the distance of closest approach for a 100 keV boron atom on silicon for an impact parameter, b = 1 nm. What is the significance of your answer? 1 MeV Al+ ions are accelerated toward a pure Ni target. The ions are directed normal to the sample surface. a) Calculate the total path length and provide an estimate for the mean projected range of the ions. b) For a dose of 1016 ions/cm2 , estimate the maximum Al concentration and the FWHM of the Al distribution. Use Se = kE 1/2 , where k = 2 × 10−16 eV1/2 cm2 . A 10 MeV Si ion penetrates a Si crystal. a) Calculate its energy as a function of distance traveled and its penetration depth. Assume that electronic stopping dominates. b) Write an expression for the depth distribution of implanted Si ions and give the straggling. Calculate the energy threshold above which the Rutherford scattering cross section can be used for: (i) near head-on collisions, and (ii) all collisions of He++ and H+ in Si and Pd. 2 MeV He++ ions are backscattered (θ = 180◦ ) off of a 25 nm thick gold foil. Determine the highest and lowest energy values of the backscattered ions as measured in a detector placed at 180◦ with respect to the incoming beam. Use k = 0.14 × 10−15 eV1/2 cm2 . Determine the stopping power by interpolation or extrapolation based on the following values of 1/N( dE/ dx) (in eV/(1015 atoms/cm2)): Energy (MeV): 1.6 2.0 Au 122.3 115.5 Al 47.5 44.25 Assume the stopping power can be described by the following function: S = C + KE 1/2

where C and K are constants.

References

1.20 1.21

1.22

1.23

71

a) Derive an equation for the particle range as a function of energy. b) Does the range increase or decrease as: i) Energy increases ii) K increases iii) C increases. Which increases the high-energy electronic stopping power the most, increased charge, energy, or mass of the projectile ion? A 2 MeV proton travels through lead. a) Assuming elastic collisions, calculate the maximum energy that can be transferred from the proton to the lead. b) What energy would a Pb ion need to have the same maximum energy transfer in a Pb–Pb collision as the proton–Pb collision in part (a)? An Fe particle is fired at a block of natural uranium. To get the Fe as close to the uranium particle as possible, would you be better off using a higher charge state of Fe or a lighter isotope? Assume Coulomb potentials can be used. A thin film containing F19 is bombarded with 1.85 MeV protons. The following reaction takes place: F19 + p → O16 + α .

The reaction has a Q value of 8.13 MeV. After interaction, an alpha particle is seen to emerge at a right angle to the incident proton beam. What are the energies of the alpha particle and the oxygen atom? What is the maximum energy each of these particles could transfer to a stationary Fe atom? 1.24 A helium atom at 1 MeV is sent into iron. Assuming the electronic stopping cross section is a constant 88 eV/(1015 atoms/cm2 ), what is the energy of the helium atom after it travels 500 nm? If the He atom collides with an Fe atom after traveling 500 nm, what is the maximum energy transferred? Assume an atomic density of 8.5 × 1022 atoms/cm3 for Fe. Was an assumption of constant stopping power valid?

References 1. Ullmaier H, Schilling W (1980) Radiation damage in metallic reactor materials. In: Physics of Modern Materials, vol. I. IAEA, Vienna 2. Lamarsh JR (1971) Introduction to Nuclear Reactor Theory. Addison-Wesley, Reading, MA 3. Doran DG (1977) Nucl Sci Eng 49:130 4. Odette GR (1972) Trans Am Nucl Soc 15:464 5. Segev M (1971) Inelastic Matrices in Multigroup Calculation, ANL-7710. Argonne National Lab, Argonne, IL, p 374 6. Evans RD (1955) The Atomic Nucleus. McGraw-Hill, New York 7. Chadderton LT (1965) Radiation Damage in Crystals. Methuen, London

72 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20.

1 The Radiation Damage Event Born M, Mayer JE (1932) Z Physik 75:1 Firsov OB (1957) Zh eksper. teor. Fiz 32:1464 Firsov OB (1957) Zh eksper. teor. Fiz 33:696 Brinkman JA (ed) (1962) Radiation Damage in Solids. Academic, New York Abrahamson AA (1963) Phys Rev 130:693 Thompson MW (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge Lindhard J, Nielsen V, Scharff M (1968) Approximation method in classical scattering by screened Coulomb fields. Mat. Fys. Medd. Dan Vid. Selsk. 36(10) Winterbon KB, Sigmund P, Sanders JB (1970) Spatial distribution of energy deposited by atomic particles in elastic collisions. Mat. Fys. Medd. Dan Vid. Selsk. 37(14) Lindhard J, Scharff M, Schiott HE (1963) Range concepts and heavy ion ranges. Mat. Fys. Medd. Dan Vid. Selsk. 33(14):3 Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge Ziegler JF, Biersack JP, Littmark U (1996) The Stopping and Range of Ions in Solids. Pergamon, New York Lindhard J, Winther A (1964) Mat. Fys. Medd. Dan Vid. Selsk. 34:1 Littmark U, Ziegler JF (1980) Handbook of Range Distributions of Energetic Ions in all Elements. Pergamon, New York

2 The Displacement of Atoms

2.1 Elementary Displacement Theory The struck lattice atom of energy T , is referred to as a primary knock-on atom, or PKA. This atom moves through the lattice encountering other lattice atoms. Such encounters may result in sufficient energy transfer to displace this lattice atom from its site resulting in two displaced atoms. If this collision sequence continues, a series of tertiary knock-ons is produced resulting in a collision cascade. A cascade is a spatial cluster of lattice vacancies and atoms residing as interstitials in a localized region of the lattice. Such a phenomenon can have a profound effect on the physical and mechanical properties of the alloy, as will become evident later. Here we are concerned with being able to quantify the displacement cascade. That is, for a neutron of energy Ei , striking a lattice atom, how many lattice atom displacements will result? We have already discussed in detail the nature of neutron–nucleus and atom–atom collisions. Now, we will develop a model for determining the number of atoms displaced by a PKA of energy T . Recall that to quantify radiation damage, we require a solution to the damage rate equation: Rd = N

Eˆ Eˇ

φ (Ei ) σD (Ei ) dEi ,

(2.1)

where N is the lattice atom density, φ (Ei ) is the energy-dependent particle flux and σD (Ei ) is the energy-dependent displacement cross section. The displacement cross section is a probability for the displacement of lattice atoms by incident particles:

σD (Ei ) =

Tˆ Tˇ

σ (Ei , T ) ν (T ) dT ,

(2.2)

where σ (Ei , T ) is the probability that a particle of energy Ei will impart a recoil energy T to a struck lattice atom, and ν (T ) is the number of displaced atoms resulting from such a collision. Chapter 1 provided the energy transfer cross section appearing in Eq. (2.2) for various types of particles in various energy ranges. This chapter will be devoted to supplying the second term in the integrand, ν (T ), the number of atom displacements resulting from a primary recoil atom of energy T , and the limits of T between which displacements occur. Finally, we will develop the displacement cross section and an expression for the displacement rate.

74

2 The Displacement of Atoms

2.1.1 Displacement Probability As a first step, we define Pd (T ) as the probability that a struck atom is displaced upon receipt of energy T . Clearly, there is some minimum energy that must be transferred in order to produce a displacement. We will call this energy, Ed . The magnitude of Ed is dependent upon the crystallographic structure of the lattice, the direction of the incident PKA, the thermal energy of the lattice atom, etc. These considerations will be discussed in detail later. By definition of Ed , the probability of displacement for T < Ed is zero. If Ed is a fixed value under all conditions then the probability of displacement for T > Ed is one. Hence our simplest model for the displacement probability is a step function: Pd (T ) = 0 =1

for T < Ed for T > Ed .

(2.3)

and is shown in Fig. 2.1. However, Ed is not constant for all collisions due to the factors mentioned earlier. The effect of atomic vibrations of the lattice atoms would be expected to lower the value of Ed or introduce a natural “width” of the order kT to the displacement probability. Further, as will be discussed later, the effect of crystallinity will also contribute strongly to the blurring effect on Ed . In fact, the picture in Fig. 2.1 and Eq. (2.3) is only strictly true for an amorphous solid at 0 K. A more realistic representation is shown in Fig. 2.2 and is represented as: Pd (T ) = 0 = f (T ) =1

for T < Edmin for Edmin < T < Edmax for T > Edmax ,

(2.4)

where f (T ) is a smoothly varying function between 0 and 1. Given the displacement probability, the next task is to find the number of displacements as a function of the energy transferred. Kinchin and Pease [1] developed a simple theory to find the average number of displaced atoms initially created by a PKA of energy T in a given solid lattice. Their analysis is based on the following assumptions:

Fig. 2.1. The displacement probability Pd (T ) as a function of the kinetic energy transferred to a lattice atom, assuming a sharp displacement threshold

2.1 Elementary Displacement Theory

75

Fig. 2.2. The displacement probability as a function of the kinetic energy transferred to the lattice atom allowing for a blurring of the threshold due to atomic vibrations, impurity atoms, etc.

1. The cascade is created by a sequence of two-body elastic collisions between atoms. 2. The displacement probability is 1 for T > Ed as given by Eq. (2.4). 3. When an atom with initial energy T emerges from a collision with energy T and generates a new recoil with energy ε , it is assumed that no energy passes to the lattice and T = T + ε . 4. Energy loss by electron stopping is given by a cut-off energy Ec . If the PKA energy is greater than Ec no additional displacements occur until electron energy losses reduce the PKA energy to Ec . For all energies less than Ec electronic stopping is ignored, and only atomic collisions occur. 5. The energy transfer cross section is given by the hard-sphere model. 6. The arrangement of the atoms in the solid is random; effects due to crystal structure are neglected. Assumption 1 is fundamental to all theories of a cascade consisting of isolated point defects. Elimination of this restriction allows the cascade to be represented by a displacement spike discussed in Chapt. 3. Assumption 2 neglects crystallinity and atomic vibrations, which will add a natural width or “blurring” effect to the distribution. Later on, we will relax Assumptions 3, 4, 5 and 6. 2.1.2 The Kinchin and Pease Model for Atom Displacements Consider the two moving atoms created when a PKA first strikes a stationary atom. After the collision, the PKA has residual energy T − ε and the struck atom receives an energy ε − Ed , giving:

ν (T ) = ν (T − ε ) + ν (ε − Ed) ,

(2.5)

where Ed is the energy consumed in the reaction. By neglecting Ed relative to ε , i.e., ε Ed according to Assumption 3, then Eq. (2.5) becomes:

ν (T ) = ν (T − ε ) + ν (ε ) .

(2.6)

76

2 The Displacement of Atoms

Equation (2.6) is not sufficient to determine ν (T ) because the energy transfer ε is unknown. Since the PKA and lattice atoms are identical, ε may lie anywhere between 0 and T . However, if we know the probability of transferring energy in the range (ε , dε ) in a collision, we can multiply Eq. (2.6) by this probability and integrate over all allowable values of ε . This will yield the average number of displacements. Using the hard-sphere Assumption 5 the energy transfer cross section is:

σ (T, ε ) =

σ (T ) σ (T ) = γT T

for like atoms ,

(2.7)

and the probability that a PKA of energy T transfers energy in the range (ε , dε ) to the struck atom is: dε σ (T, ε ) dε = , (2.8) σ (T ) T and for γ = 1 (like atoms). Multiplying the right hand side of Eq. (2.6) by dε / dT and integrating from 0 to T yields:

1 T [ν (T − ε ) + ν (ε )] dε T 0

T T 1 = ν (T − ε ) dε + ν (ε ) dε . T 0 0

ν (T ) =

(2.9)

A change in variables from ε to ε = T − ε in the first integral and Eq. (2.9) gives:

1 T 1 T ν (ε ) dε + ν (ε ) dε , T 0 T 0 which is really a sum of two identical integrals. Therefore:

ν (T ) =

ν (T ) =

2 T

T 0

ν (ε ) dε .

(2.10)

(2.11)

Before solving Eq. (2.11), let us examine the behavior of ν (ε ) near the displacement threshold, Ed . Clearly when T < Ed there are no displacements and:

ν (T ) = 0 for 0 < T < Ed .

(2.12)

If T is greater than Ed but less than 2Ed , two results are possible. The first is that the struck atom is displaced from its lattice site and the PKA, now left with energy less than Ed , falls into its place. However, if the original PKA does not transfer Ed , the struck atom remains in place and no displacement occurs. In either case, only one displacement in total is possible from a PKA with energy between Ed and 2Ed , and:

ν (T ) = 1 for Ed < T < 2Ed .

(2.13)

Using Eqs. (2.12) and (2.13) we may split the integral in Eq. (2.11) into ranges from 0 to Ed , Ed to 2Ed , and 2Ed to T and evaluate:

E 2Ed T d 2 ν (T ) = 0 dε + 1 dε + ν (ε ) dε , T 0 Ed 2Ed

2.1 Elementary Displacement Theory

77

yielding:

ν (T ) =

2Ed 2 + T T

T 2Ed

ν (ε ) dε .

(2.14)

We can solve Eq. (2.14) by multiplying by T and differentiating with respect to T giving: T

dν =ν , dT

(2.15)

with the solution:

ν = CT .

(2.16)

Substituting Eq. (2.16) into Eq. (2.14) gives: C=

1 , Ed

(2.17)

and therefore:

ν (T ) =

T 2Ed

for 2Ed < T < Ec .

(2.18)

The upper limit is set by Ec (Assumption 4). When a PKA is born with T > Ec , the number of displacements is ν (T ) = Ec /2Ed for T > Ec . So the full Kinchin–Pease (K–P) result is: ⎧ ⎪ 0 for T < Ed ⎪ ⎪ ⎪ ⎪ 1 for Ed < T < 2Ed ⎪ ⎨ T ν (T ) = (2.19) for 2Ed < T < Ec . ⎪ 2Ed ⎪ ⎪ ⎪ ⎪ E ⎪ ⎩ c for T ≥ Ec 2Ed

Fig. 2.3. The number of displaced atoms in the cascade as a function of the PKA energy according to the model of Kinchin and Pease

78

2 The Displacement of Atoms

Note that T /2Ed is a true average since the number of displacements can range from 0 (no energy transfers above Ed ) to T /Ed − 1 (every collision transfers just enough) and for large T , ν approaches T /Ed . So the maximum value of ν (T ) is 2(T /2Ed) = T /Ed . The full displacement function described by Eq. (2.19) is shown in Fig. 2.3. 2.1.3 The Displacement Energy A lattice atom must receive a minimum amount of energy in the collision in order to be displaced from its lattice site. This is the displacement energy or displacement threshold, Ed . If the energy transferred, T , is less than Ed , the struck atom will vibrate about its equilibrium position but will not be displaced. These vibrations will be transmitted to neighboring atoms through the interaction of their potential fields and the energy will appear as heat. Hence, the potential fields of the atoms in the lattice form a barrier over which the stuck atom must pass in order to be displaced. This is the source of the displacement threshold energy. Since metals are crystallographic in structure, the potential barrier surrounding an equilibrium lattice site is not uniform in all directions. In fact, there are directions in which the surrounding atoms will remove large amounts of energy from the struck atom yielding a high potential barrier. Along directions of high symmetry there exist open directions along which the threshold displacement energy is low. Since the direction of the recoil is determined from the collision event which is itself a random process, the recoil direction is entirely random. The single value often quoted for displacement energy in radiation damage calculations then represents a spherical average of the potential barrier surrounding the equilibrium lattice site. The value of Ed may be roughly estimated using an argument by Seitz [2]. The energy of sublimation, Es , for most metals is about 5 – 6 eV. Since half as many bonds are broken by removing an atom from the surface of a crystal as opposed to the interior, the energy to remove an atom from the interior is then 10 – 12 eV. If an atom is moved from its lattice site to an interstitial position in the direction of least resistance and time is allowed for neighboring atoms to relax (an adiabatic movement), an energy of 2Ec is needed. Since in reality, the struck atom is not always projected in the direction of least resistance and time is not allowed for the relaxation of neighboring atoms, a greater amount of energy (perhaps 4–5 Ec ) is needed. Thus we would expect Ed to be 20 – 25 eV. Accurate determinations of the displacement energy can be made if the interaction potential between lattice atoms is known. This is accomplished by moving the atom in a given direction and summing the interaction energies between the moving atom and all other nearest neighbors along the trajectory of the struck atom. When the total potential energy reaches a maximum, the position corresponds to a saddle point and the difference between the energy of the atom at the saddle point, E ∗ , and its energy in the equilibrium position, Eeq , represents the displacement threshold for the particular direction. Since the interaction energy in these collisions is only tens of eV, the Born–Mayer potential would be the most appropriate potential to use in

2.1 Elementary Displacement Theory

79

describing the interaction. These calculations can be carried out over all directions and averaged to obtain a mean Ed for a particular solid. To appreciate the significance of the variation in interaction energies or potential barriers with crystal direction we will consider the case of copper. In the cubic lattice there are three crystallographic directions that may be considered easy directions for displacement; 100, 110 and 111. In particular, 110 is the closepacked direction in the fcc lattice and 111 is the close-packed direction in the bcc lattice. Figure 2.4 shows how an atom is displaced along each of these directions in the fcc lattice. In each case, the displaced atom K passes through the midpoint of a set of “barrier atoms” B, in the direction of the L atom, with the atom configuration dependent on the direction. For a K atom displaced in the 110 direction, the atoms are located at the corners of a rectangle to which the path of K is perpendicular. When the K atom passes through the barrier, it loses kinetic energy in glancing collisions, which initially becomes potential energy of the barrier atoms. The energy need not be shared equally between the four B atoms. This is illustrated by drawing a set of contours of constant Ed in the place of the B atoms (Fig. 2.5). Then if K only receives a quantity of energy Ed 110 in the collision event, it will be displaced if its initial direction is contained within a small cone of solid angle centered about the 110 direction. For small energies, the cone intersects the B atom plane in a circle but as the energy transferred increases, the intersection deviates significantly from a right circular cone (Fig. 2.5). The contours are in fact, generated by the intersection of a complex but symmetrical three-dimensional surface with a sphere which is described about the atom K as center. This contour pattern can be constructed by accounting for the interaction between the K atom

Fig. 2.4. Struck atom, K, and barrier atoms B for various directions of the struck atom in the fcc lattice

80

2 The Displacement of Atoms Fig. 2.5. Equipotential contours in the barrier plane for a struck atom, K, traveling close to the 110 direction and heading toward the barrier plane defined by the barrier atoms, B (after [3])

and each of the B atoms at every point in time while simultaneously accounting for interactions between each of these five atoms and other atoms in the surrounding region of the crystal. This is a very difficult problem, the solution of which depends heavily on the interaction potential. In principle, at least, we can obtain all the information we need about the directional dependence of the thresholds. Figure 2.6 shows the displacement threshold as a function of direction in fcc copper and gold. Note that displacement threshold energies along 100 and 110 are low, but the value along 111 is high due to the large distance between barrier atoms in this direction and the two sets of barriers between the atoms on the body diagonal of the unit cell. This dependence will be further illustrated in an example using the fcc lattice and a parabolic repulsion function. Figure 2.7 shows a lattice atom on the face of a unit cell in an fcc crystal receiving energy from a collision. Its flight trajectory is in the 100 direction, which is equidistant from four atoms located on the faces of the unit cell. In an fcc lattice, each atom is surrounded by 12 nearest neighbors. Displacement will be dependent on several important factors. They are the number of barrier atoms, B, the impact parameter, z (the distance of closest approach to the B atoms), and the distance from the K atom in its lattice site to the barrier, y. These quantities are given in Table 2.1 for the fcc lattice. The energy required to displace an atom will increase with B and y and decrease with z. Since z is smallest for the 111 direction, this will be the most difficult to penetrate. Also z100 < z110 and y100 > y110 , so both factors will make displacement along 110 easier then along 100. Lets take the specific example of displacement in the 100 direction of the fcc example and calculate a value for Ed . The energy of a single atom in a normal lattice site is: Eeq = −12U ,

(2.20)

2.1 Elementary Displacement Theory

81

Fig. 2.6. Displacement energy as a function of direction in (a) fcc Cu and Au crystal (after [3]), and (b) in copper (after [4])

where U is the energy per atom of the crystal. Since only half as many bonds are broken in the sublimation process, this energy is just: Es ∼ = 6U ,

(2.21)

and since Es ∼ 4 – 5 eV, U is about 1 eV. To describe the interaction of the lattice atoms as they are pushed together in the solid, we will use a simple parabolic repulsion as opposed to the Born–Mayer

82

2 The Displacement of Atoms

Fig. 2.7. Displacement of a lattice atom along the 100 direction in the fcc lattice and the variation of energy of the atom with position along its path (after [5])

potential: 1 V (r) = −U + k(req − r)2 2 V (r) = 0 r > req ,

r < req (2.22)

where k is the force constant characterizing the repulsive position of the potential. The force constant can be expressed as [5]: ka2 =

3v , β

(2.23)

where k a v = a3 /4 β

= force constant = lattice constant = specific volume of an atom = compressibility.

In our example, the equilibrium spacing of the struck atom and the four atoms form√ ing the square barrier is req = a/ 2. When the atom is at the center of the square, it interacts with the four atoms at the corners a distance a/2 away. Hence, the energy Table 2.1. Parameters used for the determination of Ed in the fcc lattice Direction

# B atoms

Impact parameter, z

Distance to barrier, y

100

4

a 2 √

110

4

111

3

a 2√ 2 a 4 a 3

6 a 4 a √ 6

2.1 Elementary Displacement Theory

83

Table 2.2. Recommended values of the effective displacement energy for use in displacement calculations (from [6]) Metal

Lattice (c/a)

Al Ti V Cr Mn Fe Co Ni Cu Zr Nb Mo Ta W Pb Stainless steel

fcc hcp (1.59) bcc bcc bcc bcc fcc fcc fcc hcp bcc bcc bcc bcc fcc fcc

Ed,min (eV)

Ed (eV)

16 19 – 28 – 20 22 23 19 21 36 33 34 40 14

25 30 40 40 40 40 40 40 30 40 60 60 90 90 25 40

at the saddle point is:

1 1 2 1 2 = 4 −D + (ka ) √ − . E = 4V 2 2 2 2 ∗

a

(2.24)

The displacement energy in the 100 direction is then: 1 1 2 . Ed 100 = ε ∗ − εeq = 8D + 2 ka2 √ − 2 2

(2.25)

Typical values for ka2 and U for metals are 60 eV and 1 eV, respectively, yielding Ed 100 ∼ = 13.1 eV. This value is in reasonable agreement with that given in Fig. 2.6. Table 2.2 gives values of Ed for various metals [6]. Note that for the transition metals, the accepted value of Ed is 40 eV. 2.1.4 The Electron Energy Loss Limit Now that we have established a lower limit on the energy transfer necessary to cause a displacement, Ed , lets turn our attention to the high-energy regime of collisions. Recall that at low energies (T < 103 eV), Sn Se , and we may assume that nearly all of the energy loss of the PKA goes toward elastic collisions (Fig. 1.18). However, as the PKA energy increases, the fraction of the total energy loss that is due to electron excitation and ionization increases until above the crossover energy, Ex , Se > Sn .

84

2 The Displacement of Atoms

Fig. 2.8. Energy loss from electronic and nuclear stopping as a function of energy (after [7])

Our expression for ν (T ) in Eq. (2.19) must therefore be modified to account for this variation in the amount of kinetic energy available for displacement collisions. Figure 2.8 shows ( dE/ dx)n for carbon recoils in graphite using Eq. (1.162) and Lindhard’s Thomas–Fermi result, the latter showing that Eq. (1.162), which predicts a constant value of 250 eV/nm is a good approximation for energies up to at least Ea . Note that at high energies (T Ex ) electronic energy losses predominate by several orders of magnitude. However at low energies (T Ex ) the situation is reversed. Fortunately, because of departures from the hard-sphere model, the primary re1 coil creates secondaries with average energies far below Tˆ . These will almost 2 always be in the range where electronic excitation can be neglected. To obtain ν (T ) to a fair approximation we calculate the energy Ec , dissipated in elastic collisions by the PKA: Ec =

Tˇ 0

( dE/ dx)n dE . ( dE/ dx)n + ( dE/ dx)e

(2.26)

We can then use Eq. (1.182) for ( dE/ dx)e and Eq. (1.130) for ( dE/ dx)n with Tˇ = Ea . The modified damage function is the original Eq. (2.19) with T replaced by Ec :

ν (T ) =

Ec . 2Ed

(2.27)

2.2 Modifications to the K–P Displacement Model

85

Fig. 2.9. Number of displaced atoms per primary recoil compared to the simple K–P result of T /2Ed (after [7])

As an estimate of Ec we can use the maximum energy a moving atom (of energy E) can transfer to an electron as: 4me E, M

(2.28)

and equating this with the ionization energy of the struck electron belonging to the target atom we have: Ec =

M I. 4me

(2.29)

Kinchin and Pease [1] equated Ec and Ex , implying that all energy above Ex is lost in electron excitation, and displacements account for all the energy loss below Ec . Figure 2.9 shows ν (T ) for graphite using Lindhard’s ( dE/ dx)n . Note that for recoils with energy below Ec , the simple theory gives a fair description, but for T > Ec , the losses in electron excitation are important.

2.2 Modifications to the K–P Displacement Model 2.2.1 Consideration of Ed in the Energy Balance Snyder and Neufeld [8] make the assumption that an energy Ed is consumed in each collision such that the relation in Assumption 3 of the K–P displacement model will

86

2 The Displacement of Atoms

read: T = T + ε + Ed ,

(2.30)

and both atoms move off after collision, no matter how small their energy. When compared with the Kinchin–Pease model, it may be expected that ν (T ) would decrease since an energy loss term is added. However, because atoms are allowed to leave the collision with energy less than Ed , an increase in ν (T ) will occur. Since these two changes to ν (T ) nearly cancel, the result is very similar to the K–P model: T ν (T ) = 0.56 1 + (2.31) for T > 4Ed . Ed 2.2.2 Realistic Energy Transfer Cross Sections The weakest point of the K–P displacement model is the assumption of hard-sphere collisions (Assumption 5). In fact, more realistic energy transfer cross sections can be used while still maintaining the proportionality of Eq. (2.19). Sanders [9] solved Eq. (2.5) using an inverse power potential (r−s ) to obtain: 1

T ν (T ) = s 2 s+1 − 1 , 2Ed

(2.32)

which for the inverse square potential becomes:

ν (T ) = 0.52

T , 2Ed

(2.33)

reducing the Kinchin–Pease result by a factor of 2. However, the use of this potential has its shortcomings because it is applied to all collisions in the cascade while its region of validity is limited to those values of T such that ρ < 5a. Physically, the effect of realistic scattering is to make a larger number collisions generate T in the subthreshold regions below Ed where they are removed from multiplication chain. For many years, investigators have been intrigued that Eq. (2.19) appears to overestimate ν (T ) in metals by a factor of 2 to 10 [10] and yet attempts to measure the energy dependence of ν (T ) over a large energy range (50 – 200 keV recoil atoms in gold) gave a quadratic rather than linear relationship. In 1969 Sigmund [11] took a different approach to this problem by considering the recoil density F(T, ε ) dε defined as the average number of atoms recoiling with an energy in (ε , ε + dε ) as a consequence of a primary ion slowing down from T to zero energy. The recoil density can be expressed in a form that uses the power law approximation of the Thomas–Fermi differential cross section [12]:

σ (T, E) ∝ T −m ε −1−m ,

(2.34)

2.2 Modifications to the K–P Displacement Model

87

where 0 ≤ m ≤ 1, giving: F(T, ε ) =

T m , ψ (1) − ψ (1 − m) (ε + U)1−m ε 1+m

(2.35)

for T ε U, where

ψ (x) = d[ln Γ (x)]/ dx ,

(2.36)

U is the binding energy lost by an atom when leaving a lattice site, and Γ (x) is the gamma function or the generalized factorial function. Since a recoiling atom is displaced when ε > Ed we obtain:

ν (T ) =

T Ed

dε F(T, ε ) =

(1 + U/Ed)m − 1 T ψ (1) − ψ (1 − m) U

(2.37)

for T Ed U. The value of m is chosen in such a way [13] that σ (T, ε ) describes collisions at low energies, i.e., 2Ed ≤ T ≤ 100Ed. This constrains m ≤ 4. For m = 0, Eq. (2.37) reads:

ν (T ) =

6 T ln(1 + U/Ed) . π2 U

(2.38)

This is an upper limit for displacement processes since loss of defects by replacement collisions has been neglected. A characteristic feature of displacements in metals is the large recombination volume of an isolated point defect, of the order of 100 atomic volumes or more. Hence, Ed is the energy lost to the environment by an atom trying to escape the recombination volume. This has the consequence that in cascades, many defects are lost by replacement collisions [14]. The binding energy U is only a few eV and thus negligible as compared to Ed , reducing Eq. (2.38) to: T 6 T ν (T ) = 2 = 1.22 , (2.39) π Ed 2Ed which is about 22% greater than the result of Eq. (2.19) which accounted for replacement collisions. 2.2.3 Energy Loss by Electronic Excitation Even for E > Ec , collisions of the PKA with electrons compete for energy loss against collisions with lattice atoms. These two processes can be treated independently, and each can be represented by separate energy transfer cross sections. The formulation originally presented by Lindhard et al. [15] is summarized here as presented by Olander in [5] as a more realistic treatment of energy loss by electronic excitation (Assumption 4).

88

2 The Displacement of Atoms

As a PKA traverses a distance dx of a solid, three things may happen: (1) it collides with an electron, (2) it collides with an atom, or (3) nothing. Let pe dεe be the probability that a collision between the PKA and an electron in the interval dx transfers energy in the range (εe , dεe ) to the electron: pe dεe = N σe (T, εe ) dεe dx ,

(2.40)

where σe (T, εe ) is the energy transfer cross section from the PKA to the electron. Similarly, for a PKA and lattice atom: pa dεa = N σa (T, εa ) dεa dx ,

(2.41)

and the probability that nothing happens in dx is: po = 1 −

εe,max 0

pe dεe −

εa,max 0

pa dεa

(2.42)

= 1 − N dx[σe (T ) − σa (T )] , and εe,max , εa,max are the maximum energies transferable to an electron and atom by a PKA of energy T . We re-write the conservation equation for ν (T ) by weighting with the appropriate probability for the process by which it is created and integrating over the permissible ranges of energy transfers:

ν (T ) =

εa,max 0

+

[ν (T − εa ) + ν (εa )]pa dεa

εe,max 0

(2.43)

ν (T − εe )pe dεe + p0 ν (T ) .

Substituting for pe , pa and p0 yields: [σa (T ) + σe (T )]ν (T ) =

εa,max 0

+

[ν (T − εa ) + ν (εa )]σa (T, εa ) dεa

εe,max 0

ν (T − εe )σe (T, εe ) dεe .

(2.44)

Since the maximum energy transferred to an electron is very small compared to T , ν (T − εe ) can be expanded in a Taylor series and truncated after the second term:

ν (T − εe ) = ν (T ) −

dν εe , dT

(2.45)

and the last term in Eq. (2.44) can be written as: εe,max 0

ν (T − εe )σe (T, εe ) dεe = ν (T ) −

dν dT

εe,max 0

σe (T, εe ) dεe

εe,max 0

εe σe (T, εe ) dεe .

(2.46)

2.2 Modifications to the K–P Displacement Model

89

The first integral on the right in Eq. (2.46) is the total cross section for collisions of the PKA with the electron, and cancels the corresponding term on the left in Eq. (2.44). The second integral on the right of Eq. (2.46) is the electronic stopping power of the solid divided by the atom density. Substituting Eq. (2.46) using Eq. (2.45), we have:

Tmax ( dT / dx)e dν σ (T, ε ) = ν (T ) + [ν (T − ε ) + ν (ε )] (2.47) dε , N σ (T ) dT σ (T ) 0 where the subscript “a” on T and σ has been dropped with the understanding that these quantities refer to atomic collisions. (2.47) can be solved us Equation dE is given by Eq. (1.182), i.e., ing the hard-sphere assumption, but where dx e dE = kE 1/2 , giving: dx e

ν (T ) =

2Ed 2 + T T

T 2Ed

ν (ε ) dε −

kT 1/2 dν . σ N dT

After simplification, the final result is:

T 4k ν (T ) = 1 − , 2Ed σ N(2Ed )1/2

for T Ed ,

(2.48)

(2.49)

where k is a constant depending on the atom number density, N, and the atomic number. The term σ is the energy-independent hard-sphere collision cross section. Note that when electronic stopping is properly accounted for in the basic integral equation, the entire concept of a definite energy, Ec , separating regimes of electronic energy loss from atomic collisions can be dismissed. However, Eq. (2.49) is still plagued by the use of the hard-sphere assumption. Lindhard realized that in order to ensure that reliable predictions are obtained, a realistic energy transfer cross section must be used. Lindhard also realized that the parameter ν (T ) need not be interpreted solely as the number of displacements produced per PKA, but could be taken to be that part of the original PKA energy, which is transferred to the atoms of the lattice (rather than the electrons) in slowing down. In reality, collisions of the PKA with atoms compete with collisions with electrons. But the processes can be treated as independent events. Nevertheless, the expression for ν (T ) needs to be reformulated. According to Lindhard’s energy partitioning theory: T ν (T ) = ξ (T ) , (2.50) 2Ed where

ξ (T ) =

1 1/6 3/4 1 + 0.13(3.4εT + 0.4εT + εT )

,

(2.51)

90

2 The Displacement of Atoms

εT is a reduced PKA energy: εT =

T , 2Z 2 ε 2 /a

(2.52)

and a is the screening radius a=

0.8853a0 . Z 1/3

The damage energy efficiency function ξ (T ) is given as a function of PKA energy, T , and as a function of Z (various elements) in Fig. 2.10. In 1975, Norgett, Robinson and Torrens [17] proposed essentially this model to calculate the number of displacements, Nd according to: Nd =

κ ED κ (T − η ) = , 2Ed 2Ed

(2.53)

where T is the total energy of the PKA, η is the energy lost in the cascade by electron excitation, and ED is the energy available to generate atomic displacements by elastic collisions, and is known as the damage energy. The displacement efficiency, κ is 0.8 and is independent of M2 , T or temperature. The quantity ED is defined by: ED =

T , [1 + kNg(εN )]

(2.54)

Fig. 2.10. The effect of electronic energy losses on the energy available for atomic displacements (from [16])

2.2 Modifications to the K–P Displacement Model

91

and inelastic energy loss is calculated according to the method of Lindhard using a numerical approximation to the universal function, g(εN ): 1/6

3/4

g(εN ) = 3.4008εN + 0.40244εN + εN 1/2 1/6 Z1 kN = 0.1337Z1 A1 A2 T a εN = (A1 + A2) Z1 Z2 ε 2 2 1/3

9π 2/3 2/3 −1/2 a0 Z1 + Z2 a= 128

(2.55)

where a0 is the Bohr radius and ε is the unit electronic charge. If Ed ∼ 40 eV, then Nd = 10ED , where ED is in keV. 2.2.4 Effects of Crystallinity The analysis thus far has assumed that the cascade occurs in a solid composed of a random array of atoms. However, when the order of a crystal structure is imposed (Assumption 6), two important effects occur that can alter the number of displacements produced by a PKA; focusing and channeling. Focusing is the transfer of energy and/or atoms by near head-on collisions along a row of atoms. Channeling is the long-range displacement of atoms along open directions (channels) in a crystal structure in which an atom travels by making glancing collisions with the walls of the channel which are just rows of atoms. Both processes can result in long-range transport of interstitials away from the initial PKA or the cascade. Both processes also reduce the number of displacements per PKA, ν (T ), as calculated from the simple Kinchin–Pease model. Focusing The effects of focusing were first seen in the directional dependence of the threshold energy, Ed . In an fcc lattice, for example, displacements occur in the 100 and 110 directions with the lowest energy transfer of any crystalline direction. Since the direction of the primary knock-on is random, focusing must be possible for a sizable range of polar angles off the close packed direction. If exact head-on collision were required to produce a linear collision chain, the phenomenon would be of little practical significance since this probability is extremely low. Focusing along an atomic row can be analyzed using the hard-sphere approximation. The distance between atoms along a particular crystallographic is denoted by D. Figure 2.11 shows two atoms of such a row in which a collision sequence is initiated by the atom which was initially centered at A. This atom receives energy T and moves off at an angle θ0 to the atomic row. The dashed circle shows the atom position at the instant it strikes the next atom in the row. The radius of the colliding

92

2 The Displacement of Atoms

Fig. 2.11. The simple focusing effect assuming hard-sphere collisions

sphere, R, is obtained from the Born–Mayer potential. The impact transfers some of T to the second atom, which then moves off in the direction of the line joining P and B at an angle θ1 to the row. From Fig. 2.11 we can also show that: AP sin θ0 = PB sin θ1 .

(2.56)

If θ0 and θ1 are small, Eq. (2.56) can be approximated by: APθ0 ≈ PBθ1 ,

(2.57)

and if θ0 and θ1 are very small, then AP ≈ AB − PB = D − 2R , and since PB = 2R (D − 2R)θ0 = 2Rθ1 , and

θ0 (D − 2R) = θ1 (2R) .

(2.58) (2.59)

If we further define a focusing parameter: f ≡ θ1 /θ0 ,

(2.60)

then by Eq. (2.59): f=

D −1 . 2R

(2.61)

This permits us to write the following inequalities: for f > 1 ,

D > 4R

and |θ0 | < |θ1 |

for f < 1 ,

D < 4R

and |θ0 | > |θ1 | .

(2.62)

2.2 Modifications to the K–P Displacement Model

93

Considering further collisions, by the time the momentum pulse reaches atom n, the relation between angles is given by:

θn = f θn−1 = f 2 θn−2 = f 3 θn−3 (2.63)

: :

= f θ0 = n

D −1 2R

n

θ0 ,

or finally

θn = ( f ) θ0 = n

D −1 2R

n

θ0 .

(2.64)

This last relation shows that if D > 4R, the focusing parameter f is greater than unity so that the angles θn will increase in successive collisions. Conversely, if D < 4R, f is less than unity and the angles θn converge to zero. A set of conditions also exist under which the scattering angle θn will neither diverge nor converge after successive collisions. These are the conditions for critical focusing (θn = θn+1 = . . .) which can be determined as follows. The recoil angle of atom B can be related to the initial direction of atom A by applying the law of sines to triangle APB: D sin(π − θ0 − θ1 ) , = sin θ0 2R

(2.65)

which simplifies to: D sin(θ0 + θ1 ) . = sin θ0 2R

(2.66)

The condition for critical focusing is θ1 = θ0 . Applying this equality in Eq. (2.66) gives: sin 2θ0 D , = 2 cos θ0 = sin θ0 2R

(2.67)

and cos θ0 = cos θc =

D , 4R

or focusing will occur when cos θ0 ≤ cos θc =

D . 4R

(2.68) D and 4R (2.69)

94

2 The Displacement of Atoms

Equation (2.60) also shows that focusing of momentum is favored along rows of atoms in the hkl directions for which the separation distance Dhkl is a minimum, or the close-packed directions. If we treat the atoms as having an energy-dependent radius, we can determine the maximum possible energy for focusing at any given collision angle. The key is to allow the potential between atoms to vary with separation. The critical focusing energy, Efhkl , is defined as that energy below which f < 1, D < 4R and focusing is possible. In the hard-sphere model the relation between kinetic energy E, and 1 potential energy V (r) for a head on collision is given by Eq. (1.80) as V (2R) = E. 2 If V (r) is given in the Born–Mayer potential, Eq. (1.47), V (r) = A exp(−Br), then: E = 2A exp(−2R/B) .

(2.70)

For a head-on collision, θc = 0, so cos θc = Efc = 2A exp

−D 2B

D = 1, and we have: 4R

.

(2.71)

This means that any angle greater than zero will result in defocusing for E ≥> Ec , or that focusing at an energy Efc can only occur for θ = 0◦ . Clearly then, the critical focusing angle depends on the energy of the projectile. The relation between angle and energy is developed by writing the expression for Efc in terms of D: 2A D = 2B ln . (2.72) Efc Now, for any atom of energy T reaching a separation of 4R gives: 2A 4R = 2B ln . T

(2.73)

Combining these equations gives: ln(2A/Efc ) D = cos θc = , 4R ln(2A/T )

T < Efc .

(2.74)

Note that the condition of critical focusing can be expressed in two ways: −D : This condition gives the energy Efc for which focusing 1. Efc = 2A exp 2B occurs for a head-on collision (θc = 0). ln(2A/Efc ) : This condition gives the maximum angular deviation from 2. cos θc = ln(2A/T ) a head-on collision θc , at which a PKA of energy T can initiate a focused sequence.

2.2 Modifications to the K–P Displacement Model

95

From the first expression, it should be apparent that focusing is a function of crystallographic direction since D is a function of crystal structure. That is: −Dhkl Efhkl = 2A exp . (2.75) 2B For example, in the fcc lattice, we have: D100 = a √ 2 a D110 = 2 √ D111 = 3a 110

100

111

therefore, since D110 < D100 < D111 , we have Ef > Ef > Ef . 110 in copper and 600 eV for gold. In any Typical values for Ef are 80 eV for Ef case, Ef is much less than initial PKA energies. From the preceding discussion, it should be apparent that focusing is only applicable if a scattered atom is within an angle θc of an atomic row. Then a focused sequence can result. It is therefore important to determine the probability that the initial direction of a struck atom is within a cone of apex θc about an atomic row. For a random starting direction, the probability of generating a focused collision sequence at energy T is: Pf (T ) =

θc2 . 4

(2.76)

Expanding cos θc in Eq. (2.69) gives: 1 D , for small θc . Substituting from Eq. (2.75) gives: 1 − θc2 ≈ 2 4R 1 D Pf (T ) = 1− 2 4R or

1 ln(2A/Efc ) 1− 2 ln(2A/T )

ln(2T /Efc ) 1 . = 2 ln(Efc /2A) + ln(T /Efc )

(2.77)

Pf (T ) =

(2.78)

Since Efc /2A 1 and T /Efc ∼ 1, then: 1 ln(T /Efc ) 2 ln(Efc /A) = 0 T > Efc

Pf (T ) =

T < Efc

(2.79)

96

2 The Displacement of Atoms

For n equivalent directions in the crystal: Pf (T ) = n

ln(T /Ec ) . ln(Ec /A)

(2.80)

For example, in copper Efc ∼ 80 eV, and for A ∼ 20,000 eV, Pf (60 eV) ∼ 0.026n. For n = 12, then Pf ∼ 0.3 or 30%. Focusing refers to the transfer of energy by elastic collisions along a line, but without involving the transfer of mass. We will next discuss replacement collisions in which both energy and mass are transferred. Replacement Collisions In addition to energy transfer, mass can be transferred by replacement of the struck atom with the striking atom if the center of the first atom moves beyond the midpoint of the two atoms as they reside in the lattice. In our analysis of focusing we assumed hard-sphere collisions. However, if we assume that there is a softness to the atom, three things occur: 1. The hard-sphere model overestimates the angle of scattering for a particular impact parameter and hence the amount of focusing must be overestimated. 2. Atoms is the row feel the influence of the oncoming disturbance long before it gets there so the atom is already moving. Since D is decreased, focusing is enhanced. 3. Replacement becomes possible. Referring to Fig. 2.12, as the collision proceeds, the distance x between atoms An and An+l decreases continuously. The velocity of the center of mass (CM) is: M1 M2 VCM = 1 + 2 , M1 + M2 M1 + M2 where 1 and 2 are in the lab system. The relative speed, defined by g = 1 − 2 gives: M2 1 = VCM + g M1 + M2 M1 g, 2 = VCM + M1 + M2 and the total kinetic energy of the two particles is: KE = 1/2M1 21 + 1/2M222 , and in terms of g and VCM is: 2 + 1/2μ g2 , KE = 1/2(M1 + M2 )VCM M1 M2 where μ is the reduced mass = . The total kinetic energy is divided into M1 + M2 two parts: one due to the motion of the system and another due to the relative motion

2.2 Modifications to the K–P Displacement Model

97

Fig. 2.12. Head-on collisions in a focused chain when the interaction potential acts continuously during the collision. (a) Atom positions during the collision initiated by the atom on the left. (b) Separation of atoms An and An+1 during the collision (after [5])

of the two particles. Conservation of total energy is given as Er +V (x) = Er0 , where V (x) is the potential energy at a head-on separation distance of x, Er0 is the relative kinetic energy at infinite (initial) separation, and Er is the relative kinetic energy at any point. Rewriting the kinetic energy in terms of g gives: 1 1 2 μ g + V (x) = μ g20 2 2 and g0 = 10 , where g0 is the initial speed. This equation should be recognizable from our earlier analysis in Chap. 1, Sect. 1.2.2. Recall that at x = xmin , V (xmin ) = 1/2 μ g20, and for M1 = M2 , then g0 = 10 and V = E/2. We also assume that the interaction energy at the initial separation is V (D) 1 2 . The time rate of change of the separation distance is equal to the relative μ g 0 2 speed: dx = −g . dt

(2.81)

98

2 The Displacement of Atoms

Taking the collision time as twice the time needed to reach the distance of closest approach: tc = −2

xm dx

g

D

= −2

V (xm ) V (D)

dV , g dV / dx

(2.82)

where xm is the distance of closest approach. Since V (x) = A exp(−x/B), then dV A V = − exp(−x/B) = − , dx B B

(2.83)

and:

1/2 1 2 4 g= μ g0 − V (x) 2 M 1/2

4 E −V = 2 M E V 1/2 − =2 , 2M M

(2.84)

where μ = M/2 for like atoms and 1/2μ g20 = 1/4M210 = E/2. Substitution of Eqs. (2.83) and (2.84) into Eq. (2.82) yields:

2M 1/2 E/2 dV tc = B E V (D) V (1 − 2V/E)1/2

2M 1/2 2V (D) 1/2 tanh−1 1 − . = 2B E E

(2.85) (2.86)

Note that the definition of a hard-sphere radius has been used for the upper limit, i.e., xm is taken to be 2R(E). For V (D)/E 1, tc = B

2M E

1/2 ln

2E . V (D)

Since the speed of the center of mass is

(2.87) 10 = 2

E 2M

1/2 , the distance moved by

the CM during the collision time, tc , is: x = tc

E 2M

1/2 .

(2.88)

If x > D/2, atom An will end up to the right of the initial halfway point and replacement will occur and An will occupy the lattice site occupied by atom An+1 . Relating

2.2 Modifications to the K–P Displacement Model

99

Fig. 2.13. Energy scale for focused energy transfer and focused replacement sequence

the distance x to energy by substituting for tc from Eq. (2.87) into Eq. (2.88) gives: 2Er x = ln . (2.89) B V (D) For x = D/2: D 2Er , = exp 2B A exp(−D/B) and the replacement energy becomes: −D A Er = exp . 2 2B

(2.90)

According to the above arguments, and comparing to Eq. (2.71), focused replacement is possible when the energy transported in the collision chain satisfies: −D 1 1 = Efc . (2.91) E > Er = A exp 2 2B 4 Therefore, we get focused replacement, or Efc /4 < T < Efc : focused replacement T < Efc /4 : focused momentum/energy packet . Hence mass transfer can occur when E is between Er = Efc /4 and Efc , which from our previous example is about the same or slightly less than the displacement energy, Ed . Figure 2.13 shows where focusing and replacement collisions fall on the energy spectrum of the PKA. Assisted Focusing In our analysis of focusing, we have not accounted for the effects of surrounding atoms or nearest neighbors. Due to their repulsion of the moving atom, they tend to act as a lens and aid in the focusing process. The net result of this assisted focusing is to increase the critical energy for focusing, Efc , rendering focusing more probable. Second, the ring of atoms surrounding a focusing event also tend to dissipate energy by glancing collisions. This effect is augmented by the vibrational motion of the atom rings, which can be increased with temperature. The length of

100

2 The Displacement of Atoms

the replacement chain and the number of collisions in the chain decrease as the temperature increases. The increased motion of the surrounding atoms increases the energy loss from the collision sequence. Other effects that destroy the sequence are alloying elements and defects such as interstitials, vacancies and dislocations. Figure 2.14 shows the number of collisions in a focused chain of initial energy E in room-temperature copper along with the focusing probability. Table 2.3 from Chadderton [18] gives the focusing and replacement energies in various directions in fcc and bcc lattices as modified by surrounding atoms (assisted focusing). Note that in all cases, the focusing energies are larger when the surrounding atoms aid in the focusing process.

Fig. 2.14. Length and probability of the collision chain in a 110 collision sequence in copper at room temperature (after [5]) hkl ) in the fcc and bcc lattices (after [18]) Table 2.3a Equations for focusing energies (Efc

hkl Face-centered cubic

Body-centered cubic

↑ A(D110 )2 D110 exp − 4B 2D2 D110 110 2A exp − 2B 1/2 ↑ 6 D110 19 1/2 A(D110 )2 A 111 exp − 19 2B 12 D2

D111 2A exp − √ B 3 √ ↑↑ √ D111 5 4 2(D111 )2 A exp − √ 15B2 2 3B 111 D 2A exp − 2B

100

2.2 Modifications to the K–P Displacement Model

101

Table 2.3b Equations for replacement energies (Erhkl ) in the fcc and bcc lattices (after [18]) hkl

Face-centered cubic D110 100 5A exp − √ D 2 D110 A exp − 110 2 2B D110 111 4A exp − √ B 3 ↑ In the (110) plane only ↑↑ Assisted focusing

Body-centered cubic D100 A exp − 2 2B D110 3A exp − 2B D111 2A exp − 2B

Channeling Channeling is the long distance displacement of energetic knock-on atoms down an open direction in the crystal lattice. Figure 2.15a shows a schematic of an atom spiraling down an open channel in a crystal lattice and Fig. 2.15b shows axial and planar channels along specific crystallographic directions in the fcc lattice. The walls of the passageway consist of atomic rows. If the rows surrounding the channel are close-packed, discrete repulsive forces between atoms are “smeared out” and the atom appears to be traveling in a long cylindrical tube with radius Rch . The value of Rch can be determined by equating π R2ch with the cross sectional area of the channel. If the amplitude of the lateral oscillations of the moving atom is small compared to Rch , the potential well provided by the channel wall is roughly parabolic in the direction transverse to the channel axis. The interaction of the moving atom with a channel wall (Fig. 2.16) can be described by a harmonic channel potential: Vch (r) = kr ,

(2.92)

where r is the lateral distance from the axis, and k is the force constant which depends on the potential function describing atom–atom repulsion and channel dimension Rch . Using the Born–Mayer potential to describe atom–atom interactions in this energy regime, k becomes: −Rch A 2π Rch k= exp , (2.93) DB B B where D is the atom spacing in the rows forming the channels. Moving atoms enter the channel with a velocity component along the channel axis (Fig. 2.16) given by: 1/2 2E cos θ0 , (2.94) Vz0 = M where (2E/M)1/2 = V0 . The axial velocity is gradually reduced by inelastic energy loss to the electron cloud. The moving atom undergoes simple harmonic motion in

102

2 The Displacement of Atoms

Fig. 2.15. (a) Schematic of an atom moving in a channel in a crystal lattice (after [19]). (b) Axial and planar channels in the fcc lattice (after [20])

2.2 Modifications to the K–P Displacement Model

103

Fig. 2.16. Trajectory of a channeled atom (after [5])

the r direction with period τ given by: 1/2 M τ = 2π 2k and the initial wavelength of the oscillation is equal to Vz0 τ for θ0 = 0 or: 1/2 E λ = 2π . k

(2.95)

(2.96)

The amplitude of lateral oscillation is determined by the injection angle, θ0 and the kinetic energy of the injected atom, E. The r component of the atom velocity as it enters the channel is: 1/2 1/2 2E 2E ∼ Vr0 = sin θ0 = θ0 . (2.97) M M So the radial component of the kinetic energy is E θ02 , which is equal to the potential 2 . Equating kinetic and potential energies energy at the transverse amplitude, krmax and solving for rmax gives: 1/2 E rmax = θ0 , k and the trajectory of the channeled atom is: 1/2 1/2 k E r = θ0 sin Z . k E

(2.98)

(2.99)

104

2 The Displacement of Atoms

The critical angle beyond which channeling cannot occur, θch , is obtained by equating the transverse amplitude, rmax , and the channel radius, Rch : 1/2 k θch = Rch . E

(2.100)

Note that θch decreases as E increases, as expected. When the mean free path between collisions is of the order of a few atom spacings, large-angle collisions become probable and channeling dissipates. The channeling probability is difficult to determine since we must knock an atom into the channel, but there are no atoms near the channel axis. The event probably starts with an impact on an atom forming the channel wall. If the entrance angle is small enough, it may begin to channel. There is no upper limit on energy for channeling. Instead, θch just becomes smaller as E increases. The minimum channeling energy occurs when the wavelength is ∼ nD or a few atom spacings (n ∼ 2). Essentially, there develops a resonance between impulses from channel walls and transverse oscillations. The trajectory terminates in a violent collision. Recall that our treatment is only valid if λ D. Solving for E in Eq. (2.96) and letting λ = 2D yields Ech ∼ 0.1 kD2. For copper, Ech is about 300 eV. Ech is larger for large mass because k increases with mass. Channeling is a high-energy phenomenon and is most significant for light atoms, while focusing is a low-energy phenomenon that is most significant for heavy atoms. Effect of Focusing and Channeling on Displacements The probability of a crystal effect is a function of recoil energy. P(T ) is used for either Pf or Pch , but since Ef ∼ 100 eV, Pf is quite small. The equation governing cascade effects can be modified to account for crystal effects by modifying Eq. (2.14):

2Ed 2 T + ν (T ) = P(T ) + [1 − P(T)] ν (ε ) dε . (2.101) T T 2Ed The first term on the right in Eq. (2.101) represents the lone displaced atom, which results if the PKA is channeled or focused on the first collision. The second term gives the number of displacements created by a PKA that makes an ordinary displacement on the first collision. Assuming P = P(T ), Eq. (2.101) is differentiated with respect T to yield: T

dν = (1 − 2P)ν + P . dt

(2.102)

Integration gives

ν (T ) =

CT (1−2P) − P 1 − 2P

(2.103)

2.3 The Displacement Cross Section

105

Fig. 2.17. Energy scale showing focused energy transfer, focused replacement sequence and channeling

and the constant C can be found by substitution into Eq. (2.82): C=

1−P , (2Ed )(1−2P)

resulting in the final solution: T (1−2P) 1−P P . ν (T ) = − 1 − 2P 2Ed 1 − 2P For small P, ν (T ) can be approximated by: T (1−2P) ν (T ) = . 2Ed

(2.104)

(2.105)

It should be noted that the most important crystal effect is channeling which is most important at high energies. For example, for P = 7%, a 10 keV PKA in iron produces 100 displacements or about half the amount with P = 0. Figure 2.17 shows where channeling occurs on the PKA energy scale. Note that channeling is a high-energy phenomenon and that there is a gap between the replacement energy, below which replacements or focused energy transfer occur, and the channeling energy, above which channeling occurs. Given the K–P model for displacement and the various modifications to the basic model, we now turn to the determination of the number of displaced atoms.

2.3 The Displacement Cross Section The results of previous sections may now be used to define the displacement cross section as:

σD (Ei ) =

Tˆ Tˇ

ν (T )σ (Ei, Q j , T ) dT ,

(2.106)

106

2 The Displacement of Atoms

where ν (T ) is the number of displacements caused by a PKA of energy T , σ (Ei, Q j , T ) is the general form of the energy transfer cross section, and Tˇ and Tˆ are the minimum and maximum transfer energies. This quantity was first presented in Eq. (2.2) and gives the average number of displacements produced by an incoming neutron of energy Ei . We can apply this expression to the various regimes of scattering in order to determine their individual contributions to the total number of displacements. We will first determine σD (Ei ) for each type of interaction using the basic K–P result and then go back and add in the modifications. 2.3.1 Elastic Scattering Consider σs (Ei , T ) for elastic scattering. From Eq. (1.19),

σs (Ei , T ) =

4π σs (Ei , φ ) . γ Ei

In the case of isotropic scattering:

σs (Ei , φ ) =

σs (Ei ) ; 4π

therefore:

σs (Ei ) σDs (Ei ) = γ Ei

γ Ei Ed

σs (Ei , T ) =

σs (Ei ) , γ Ei

ν (T ) dT .

(2.107)

Should we wish to consider anisotropic elastic scattering in systems such as fast reactors, the angular dependence of the elastic scattering cross section can be written in a series of Legendre polynomials:

σs (Ei , φ ) =

σs (Ei ) ∞ ∑ a(Ei )P(cos φ ) , 4π =0

(2.108)

where σs (Ei ) is the total elastic scattering cross section for incident neutrons of energy Ei , P is the th Legendre polynomial, and values of a are the energy-dependent coefficients of the cross section expansion. At neutron energies encountered in thermal or fast reactors, it is sufficient to retain only the first two terms, = 0 and = 1. Since P0 = 1 and P1 = cos φ :

σs (Ei , φ ) =

σs (Ei ) [1 + a1(Ei ) cos φ ] . 4π

(2.109)

Also, given that cos φ = 1 − 2T /γ Ei , and substituting Eq. (2.109) into Eq. (2.106) gives:

2T σs (Ei ) γ Ei σDs (Ei ) = ν (T ) 1 + a1(Ei ) 1 − dT . (2.110) γ Ei E d γ Ei

2.3 The Displacement Cross Section

107

2.3.2 Inelastic Scattering Since inelastic scattering is isotropic in the center-of-mass system:

σs j (Ei , Q j , φ ) =

σs j (Ei , Q j ) . 4π

(2.111)

Equation (1.30) gives the energy transfer cross section for inelastic scattering in the resonance region as:

σs j (Ei , Q j ) Qi 1 + A −1/2 σs j (Ei , Q j , T ) = , 1+ γ Ei Ei A so that

σDs j (Ei ) = ∑ j

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj 1+ ν (T ) dT , γ Ei Ei A Tˇ j

(2.112)

where the minimum and maximum values of T (Ei , Q j , φ ) are given by Eq. (1.27) and setting cos φ = −1 and 1, respectively, gives: 1/2 Q Q 1 + A γ E 1 + A j j i 1+ + 1+ Tˆj = 2 2A Ei Ei A 1/2 Q Q 1 + A γ E 1 + A j j i 1+ − 1+ Tˇ j = . 2 2A Ei Ei A 2.3.3 (n, 2n) and (n, γ ) Displacements The displacement cross section for (n,2n) reactions can be written as:

σD(n,2n) (Ei ) =

Ei −E m 0

σ(n,2n) (Ei T )

T dT , 2Ed

(2.113)

where σ(n,2n) (Ei , T ) is given by Eq. (1.40). The displacement cross section due to (n, γ ) reactions can be written as:

σDγ (Ei ) = σγ

Tˆ T 0

2Ed

dT .

(2.114)

However, since we have assumed that the lattice atom recoils with an average energy T=

Eγ2 Tˆ = , 2 4(A + 1)c2

and that Eγ for a given isotope is either known or can be measured, Eq. (2.114) can be simplified to:

σDγ = σγ

Eγ2 T = . 2Ed 8Ed (A + 1)c2

(2.115)

108

2 The Displacement of Atoms

The total displacement cross section due to these forms of neutron interaction then becomes:

σD (Ei ) =σDs (Ei ) + σDs j (Ei ) + σD(n,2n) (Ei ) + σDγ

2T σs (Ei ) γ Ei T = 1 + a1(Ei ) 1 − dT γ Ei Ed 2Ed γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T dT +∑ 1+ γ Ei Ei A Tˇ j 2Ed j +

Ei −E m 0

+ σγ

σ(n,2n) (Ei , T )

Eγ2 , 8Ed (A + 1)c2

T dT 2Ed (2.116)

where the terms are for elastic scattering, inelastic scattering in the resonance region, (n,2n) reactions and (n,γ ) reactions, respectively. 2.3.4 Modifications to the K–P Model and Total Displacement Cross Section The displacement cross section can be modified to account for the relaxation of the various assumptions made to the basic K–P model as in Sect. 2.2. These modifications are as follows summarized in Table 2.4. Applying these correction terms to the basic K–P result by consolidating Assumptions 1 and 3 into a single constant C and using Eq. (2.104) for the effect of crystallinity, transforms Eq. (2.116) to read: σs (Ei ) γ Ei 1 − P T (1−2P) P σD = − C ξ (T ) γ Ei E d 1 − 2P 2Ed 1 − 2P

2T × 1 + a1(Ei ) 1 − dT γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 +∑ 1+ γ Ei Ei A j Tˆj T (1−2P) P 1−P dT × − C ξ (T ) 1 − 2P 2Ed 1 − 2P Tˇ j Ei −E m 1−P T (1−2P) P + dT σ(n,2n) (Ei , T ) − C ξ (T ) 1 − 2P 2Ed 1 − 2P 0 ⎤ ⎡ 1−2P 2 E 1−P P ⎦ γ + σγ ⎣ . (2.117) C ξ (T ) − 1 − 2P 8Ed (A + 1)c2 1 − 2P

2.4 Displacement Rates

109

Table 2.4. Modifications to the displacement cross section Assumption 3: Loss of Ed 4: Electronic energy loss cut-off 5: Realistic energy transfer cross section 6: Crystallinity

Correction to ν (T ) T 0.56 1 + 2E d T ξ (T ) 2Ed T , 0.52 < C ≤ 1.22 C 2Ed 1−P P T (1−2P) − 1 − 2P 2Ed 1 − 2P T (1−2P) ∼ 2Ed

Equation in text Eq. (2.31) Eq. (2.50) Eqs. (2.33), (2.39)

Eq. (2.104) Eq. (2.105)

Using the more simplified expression for the effect of crystallinity Eq. (2.104) reduces Eq. (2.117) to: (1−2P)

σs (Ei ) γ Ei T 2T σD = C ξ (T ) 1 + a1(Ei ) 1 − dT γ Ei E d 2Ed γ Ei

σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T (1−2P) dT +∑ 1+ C ξ (T ) γ Ei Ei A 2Ed Tˇ j j Ei −E m T (1−2P) + σ(n,2n) (Ei , T ) C ξ (T ) dT 2Ed 0 1−2P Eγ2 , (2.118) + σγ C ξ (T ) 8Ed (A + 1)c2 or,

σD = σDs + σDi + σD(n,2n) + σDγ .

(2.119)

The displacement cross section for stainless steel was calculated by Doran [21] using the energy partition theory of Lindhard and is shown in Fig. 2.18.

2.4 Displacement Rates Recall that the displacement rate was given in Eq. (2.1) as: R=

Tˆ Tˇ

N φ (Ei )σD (Ei ) dEi .

This is the displacement rate density or total number of displacements per unit volume per unit time [#/cm3 s]. To get a rough estimate of the order of magnitude of

110

2 The Displacement of Atoms

Fig. 2.18. The displacement cross section for stainless steel based on a Lindhard model and ENDF/B scattering cross sections (after [21])

this number, let us simplify the displacement cross sections as follows. Neglecting (n,2n) and (n,γ ) contributions to displacements, all modifications to the simple K–P displacement model (i.e., using ν (T ) = T /2Ed ), and neglecting Ed relative to Ei , the displacement cross section due to elastic and inelastically scattered neutrons only becomes:

2T σs (Ei ) γ Ei T σD (Ei ) = 1 + a1(Ei ) 1 − dT γ Ei Ed 2Ed γ Ei

(2.120) σs j (Ei , Q j ) Q j 1 + A −1/2 Tˆj T +∑ dT . 1+ γ Ei Ei A Tˇ j 2Ed j Assuming that elastic scattering is isotropic (a1 = 0), neglecting inelastic scattering and integrating between the limits Ed and γ Ei gives:

σD (Ei ) =

σs (Ei ) γ Ei

γ Ei T Ed

2Ed

dT ,

and if γ Ei > Ec , then:

2E Ec γ Ei d σs (Ei ) T Ec σD (Ei ) = dT + dT + dT γ Ei Ed 2Ed 2Ed Ec 2Ed

2 2 Ed σs (Ei ) (γ Ei ) 2 = − + γ Ei Ec − Ec . Ed + 2 γ Ei Ed 2 2

(2.121)

(2.122)

2.4 Displacement Rates

111

If we choose γ Ei ∼ Ec and neglecting terms in Ed or Ed2 gives:

σD (Ei ) ≈

γ Ei 4Ed

σs (Ei ) ,

(2.123)

and Eq. (2.2) becomes: Nγ 4Ed

∞

σs (Ei )Ei φ (Ei ) dEi γ E¯ i Φ, = N σs 4Ed

R=

E d /γ

(2.124) (2.125)

where E¯ i is an average neutron energy and Φ is the total neutron flux above energy Ed /γ , and the term in brackets is the number of displacements (Frenkel pairs) produced per neutron. The validity of assuming isotropic scattering and neglecting inelastic scattering is shown in Figs. 2.19 and 2.20. Essentially, both approximations are reasonable at energies below one to a few MeV.

Fig. 2.19. Recoil energy spectra from the elastic scattering of fast neutrons using data from ENDF/B files (after [22])

112

2 The Displacement of Atoms

Fig. 2.20. Displacement cross section for nickel showing the elastic and inelastic components (after [21])

Example 2.1. Neutron irradiation of iron. As an example, let us look at the damage caused by 0.5 MeV neutrons in Fe in a fast flux that may be representative of the core of a fast reactor: N = 0.85 ×1023 atoms/cm3

σs = 3 ×10−24 cm2 Φ = 1015 neutrons cm−2 s−1 γ Ei = 350 displaced atoms/neutron 4Ed R is 9 ×1016 displaced atoms per cm3 per second, or dividing R by N gives ∼ 10−6 dpa/s. This is equivalent to each atom being displaced from a normal lattice site once every 12 days. A second example can be worked for the displacement rate in the aluminum fuel plates in an MTR-type thermal neutron research reactor. In this case, we have: Ei ∼ 0.5 MeV N = 0.6 ×1023 atoms/cm3

σs = 3 ×10−24 cm2 Φ = 3 ×1013 neutrons cm−2 s−1

2.5 Correlation of Property Changes and Irradiation Dose

113

γ Ei = 690 displaced atoms/neutron 4Ed R is 4 ×1015 displaced atoms per cm3 per second, or dividing R by N gives ∼ 7 ×10−8 dpa/s, or about 2/yr. Note that even though the number of displacements per neutron is almost a factor of 2 higher in Al than in Fe, the damage rate is significantly lower because of the much lower fast flux in this type of reactor.

2.5 Correlation of Property Changes and Irradiation Dose The ultimate objective of the calculation of Rd is to provide a prediction of the extent of change of a particular property of the material under irradiation. The mechanical property may be yield strength, swelling, degree of embrittlement, etc. Recall in the Introduction that the determination of the number of displaced atoms was motivated by the inability of particle fluence to account for property changes (see Fig. I.1 in the Introduction). While an improvement over units of exposure such as neutron fluence, displacement rate alone cannot alone account for the macroscopic changes observed, and a semi-empirical method of correlating damage with macroscopic property changes has evolved known as the damage function method. In this method the atom displacement rate is replaced with the change in some macroscopic property after a time t of irradiation. The displacement cross section is replaced by the damage function for the particular mechanical property, Gi (E), hence: ΔPi j =

Gi (E)φ j (E,t) dE dt ,

(2.126)

where ΔPi j is the change in the property labeled by the index i, during an irradiation time of t and in a neutron flux where φ j (E,t) is the jth neutron differential spectrum. Assuming energy-time separability, φ j (E,t) = φ j (E)t, then Eq. (2.126) can be rewritten as: (k)

ΔPi j = t ·

(k)

Gi (E)φ j (E) dE ,

(2.127)

where the superscript refers to the kth cycle of iteration. The objective is to deduce a single function Gi (E) from a set of measured ΔPi (k) values. Given ΔPi j and φ j (E) as input along with an initial approximation of Gi (E) (0)

(k)

or Gi (E), a computer code is used to generate iterative solutions Gi (E). An appropriate solution is obtained when the standard deviation of the ratios of all (k) measured-to-calculated values ΔPi j /ΔPi j reaches a lower value that is consistent with experimental uncertainties. As it turns out, the resultant damage function is

114

2 The Displacement of Atoms

Fig. 2.21. (a) A 60 ksi yield strength damage function for 304 stainless steel irradiated and tested at 480 ◦C (after [23]). (b) Damage function for a 2.0 ×10−8 psi−1 ε¯ /σ¯ property change for stainless steel (after [24])

2.6 Displacements from Charged Particle Irradiation

115

Fig. 2.22. Dose dependence of swelling, resistivity and radiation-induced segregation

highly sensitive to the initial approximation as shown in Fig. 2.21. But note that since the shape of Gi (E) is the same as the displacement function, it is clear that they are related. However, this result tells us that we cannot fully understand radiation effects by only calculating the number of displaced atoms. We cannot treat radiation effects as a black box. Rather, in order to understand the effect of the damage on the properties of the material, we must understand the fate of these defects after they are formed. This realization is reinforced by the property dependence on dose shown in Fig. 2.22. Note that for the three property changes, resistivity, radiation-induced segregation and hardening, the functional dependence on dose is strikingly different between them. While property change certainly relates to displacement damage, the nature of the change is not uniform but varies considerably depending on the property measured. The next chapter explores the spatial and temporal distribution of radiation damage. But before we examine the damage zone in detail, let us complete our picture of the production of displacements by addressing the damage created by charged particles such as ions and electrons.

2.6 Displacements from Charged Particle Irradiation Displacements from charged particles differ from those due to neutrons because as they travel through the lattice, they lose energy via electronic excitation in addition to via elastic collisions. Figure 2.23 shows the trade-off in energy loss mechanism dominance with energy in the energy range of relevance for ion–solid interaction, and Fig. 2.24 shows the residual ion energy as a function of ion penetration depth. Note that electronic stopping will dominate at short depths, but elastic collisions

Fig. 2.23. Variation in nuclear and electronic stopping powers over the energy range of relevance to ion–solid interactions

116

2 The Displacement of Atoms Fig. 2.24. Residual range of an ion incident on a target and the regimes of electronic and nuclear stopping dominance

will dominate near the end of range. An expression for the number of displacements from a charged particle can be derived from the analysis of energy lost from the PKA by electronic excitation given in Sect. 2.2.3 and described by Eq. (2.40) through Eq. (2.49). Equation (2.44) describes the loss of energy to both atoms and electrons in the target by the PKA. We can revisit this analysis assuming that the particle we are tracking is the incident ion. As was done in Eq. (2.45), we can expand the terms for ν (T − εa ) and ν (T − εe ) in a Taylor series and truncate the series after the second term, giving: dν εa , dT dν ν (T − εe ) = ν (T ) − εe , dT

ν (T − εa ) = ν (T ) −

(2.128)

and the integrals involving the terms ν (T − εa ) and ν (T − εe ) can both be written in the general form: εmax 0

ν (T − ε )σ (T, ε ) dε = ν (T )

εmax 0

σ (T, ε ) dε −

= ν (T )σ (T ) −

dν dT

εmax

dν (T ) S(T ) . dT

0

εσ (T, ε ) dε

(2.129) Since in this treatment, the ion is the incoming projectile, we will re-write Eq. (2.129) using our established convention that the incoming particle is of energy Ei and it transfers energy T to the target atoms and electrons, and the maximum energy transfer is Tˆ : Tˆ

Tˆ

dν Tˆ ν (Ei − T )σ (Ei , T ) dT = ν (Ei ) σ (Ei, T ) dT − T σ (Ei , T ) dT dE 0 0 0 dν (Ei ) S(Ei ) , = ν (Ei )σ (Ei ) − (2.130) dE where Eq. (1.79) is used to transform the integral of the differential energy transfer cross section, σ (Ei , T ) to the total collision cross section σ (Ei ), and Eq. (1.129) is used to transform the integral of T σ (Ei , T ) into the stopping cross section S(Ei ).

2.6 Displacements from Charged Particle Irradiation

117

Applying the results of Eqs. (2.129) and (2.130) into Eq. (2.44) gives: dν (Ei ) =

dE S(Ei )

Tˆ 0

ν (T )σ (Ei , T ) dT .

(2.131)

Since we are concerned with the total number of displacements over the entire range of the ion rather than the specific number of displacements over a distance dx of the sample, we can integrate Eq. (2.131) over the entire range of ion energy loss to obtain the number of displacements resulting from an incident ion with initial energy Ei :

ν (Ei ) = =

Ei Tˆ dE

ν (T )σ (E , T ) dT

0

S(E )

0

dE , σd (E ) S(E )

Ei

Ed

(2.132)

and Tˆ Ed

ν (T )σ (E , T ) dT ≡ σd (E ) ,

(2.133)

where E = E (x) is the ion energy as a function of the traveled path length x as the ion travels down to zero energy. We can work a simple example using an approximation to the treatment given above. We are interested in the number of collisions made by an ion as it passes through a solid. We will take I as the ion flux in units of ions/cm2 and we can write the number of collisions per second in a volume element of unit cross sectional area and thickness dx which transfer energy in the range (T, dT ) to atoms of this element as: NI σ (E, T ) dx .

(2.134)

The number of collisions per unit volume per unit time which transfer energy in (T, dT ) at depth x is NI σ (E, T ) [collisions/cm3 s]. The number of displaced atoms for each collision that produces a PKA of energy T is ν (T ). Therefore, the production rate of displaced atoms at depth x is: Rd (x) = NI

γE Ed

σ (E, T )ν (T ) dT

[displacements/cm3 s] .

(2.135)

(Note that we have not accounted for the fact that I is a function of x (or E) and that I(x) = I0 .) E is a function of x since the ion slows down by loss of energy to the electrons of the target. The functional form of E(x) can be estimated using dE/ dx = kE 1/2 as: E(x) = [(Ei )1/2 − 1/2kx]2 ,

(2.136)

where Ei is the initial energy of the ion when it strikes the target. The number of dpa at a depth x is Rd (x)/NI. displaced atoms/atom/s is Rd (x)/N and the (ions/cm2 )

118

2 The Displacement of Atoms

We will assume that σ (E, T ) can be described by Rutherford scattering and using the Lindhard treatment for ν (T ) from the K–P model, and assuming ξ = 0.5 gives: γ Ei Rd 1 π Z12 Z22 ε 4 M + Mi 2 1 4Mi M 1 T = dT NI 4 M Ei (M + Mi )2 T 2 2Ed Ed 2 (2.137) π Z12 Z22 ε 4 Mi γ Ei dpa = . ln 4Ei Ed M Ed ion/cm2 Applying this result to 0.5 MeV protons in iron gives ∼ 10−18 dpa/(ions/cm2) at the surface. 20 MeV C+ ions incident on nickel produce ∼ 3 ×10−18 dpa/(ions/cm2) at the surface, but 50 times this amount at the damage peak. These values can be compared to the damage rate from 0.5 MeV neutrons in iron: Rd γ Ei = σs Nφ 4Ed (2.138) = 350 × 3 ×10−24 = 1 ×10−21

displacements . n/cm2 s

Comparing 0.5 MeV neutrons to 20 MeV C+ ions shows that over their range C+ ions produce 3000 times more displacements than do neutrons. Figure 2.25 com-

Fig. 2.25. Displacementdamage effectiveness for various energetic particles in nickel (after [25])

Nomenclature

119

pares the displacement rates as a function of penetration depth for ions of various mass and energy. As expected, for the same energy, ions of heavier mass deposit their energy over a shorter distance resulting in higher damage rates. Note that due to the large collision mean free path of a neutron as compared to an ion, the neutron damage energy is low and constant over distances of millimeters.

Nomenclature a a0 A A B B c D Ec Ech Efc Ed ED Ei Er Es Eγ Ei, Em Em E∗ Eeq f g G I¯ k m me M1 M2 N p, pe , pa Pch Pd Pf

Lattice constant Bohr radius of the hydrogen atom Atomic mass Pre-exponential constant in Born–Mayer relation, Eq. (1.47) Spacing between barrier atoms in crystal lattice Constant in exponent in Born–Mayer relation, Eq. (1.47) Speed of light Nearest neighbor spacing between atoms Cut-off energy; critical energy for focusing Critical energy for channeling Critical focusing energy Displacement energy Damage energy Projectile energy Critical energy for replacement collisions; relative kinetic energy Sublimation energy Gamma ray energy Incoming particle energy Kinetic energy of incoming particle in CM system Energy of neutron after (n, 2n) reaction Saddle point energy Energy of atom in equilibrium lattice site Focusing parameter Relative speed 1 − 2 Damage function Excitation-ionization level Force constant; constant in the electronic energy loss term, kE 1/2 Mass of incoming particle; 1/s Mass of the electron Mass of projectile Mass of target Atom number density Probability, refers to electron, refers to atom Channeling probability Displacement probability Focusing probability

120

2 The Displacement of Atoms

Q req rmax R Rch Rd S S, Se , Sn tc T Tˇ Tˆ T¯ T U V V (r) ν VCM 1 2 VCM Y z Z

Excitation energy of nucleus Equilibrium spacing between atoms Transverse amplitude of channeled atom Atomic radius Radius of channel Displacement rate [#/cm3 s] Exponent in the power law approximation Stopping power; electronic; nuclear Collision time Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy transferred to target atom after (n,2n) reaction Energy per atom in a crystal Energy per atom in a crystal Potential energy Specific volume of the atom Velocity of CM in lab system Velocity of projectile in lab system Velocity of target in lab system Velocity of center of mass Distance to atom barrier Impact parameter Atomic number

β ε εeq ε ε∗ φ,Φ γ η κ μ ν ν (T ) θ θc θch σ (Ei ) σ (Ei , T ) σD σs

Compressibility Secondary atom knock-on energy; unit charge Eq. (2.52) Energy of atom in a normal lattice site Reduced PKA energy Energy of atom at saddle point Neutron flux 4M1 M2 /(M1 + M2 )2 Energy lost to electronic excitation in the NRT model Displacement efficiency Reduced mass specific volume of an atom Displacement function Scattering angle in lab system Critical focusing angle Critical channeling angle Total atomic collision cross section Differential energy transfer cross section Displacement cross section Scattering cross section

Problems

σs j σ(n,2n) σγ τ ξ

121

Inelastic scattering cross section for the jth resonance Cross section for (n,2n) reactions Cross section for (n,γ ) reactions Period for oscillation for a channeled atom Damage energy efficiency, Eq. (2.50)

Problems 2.1 a) Using the simple K–P model and assuming only elastic, isotropic scattering, calculate the number of displacements per atom (dpa) in nickel subjected to a fast neutron (2 MeV) fluence of 1022 n/cm2 . b) Using the relativistic expression for the electron–atom energy transfer, calculate the minimum electron energy required to displace an atom in (i) Al and (ii) W. 2.2 In a (n, 2n) reaction, a second neutron can only be emitted if the residual excitation of the nucleus after emission of the first neutron exceeds the binding energy of a neutron in the mass M nuclide. The recoil energy after emission of the first neutron is taken to be the average value (cos φ = 0). Write an expression for the recoil energy following the second emission. 2.3 An 56 Fe nucleus undergoes an (n,γ ) reaction resulting in the release of a single 7 MeV gamma ray, on average. If a steel component is located in a reactor where the peak thermal flux is 1×1014 n/cm2 and the thermal/fast flux ratio is fast ≥ 1 MeV), determine the relative displacement rates by fast one (where Eave neutrons, recoil nuclei and gamma rays which undergo Compton scattering. Assume σ(n,γ ) ∼ 4b, σs ∼ 3b. 2.4 A slab of iron is exposed to a 20 MeV gamma source. a) What is the most probable interaction between the gamma and the electrons in the Fe? b) Assume the reaction you chose in part (a) occurs. Can this lead to the displacement of an Fe atom if the displacement energy is 40 eV? 2.5 A thermal neutron causes the following reaction 27

Al + n → 28 Al + γ .

The gamma energy is 1.1 keV. The gamma will interact with lattice electrons. What is the most probable event? For this event, what is the maximum energy transferred? Does the resultant electron have enough energy to displace an aluminum atom (assume the displacement energy is 25 eV). Can the recoil Al atom displace another aluminum atom? 2.6 The (n,γ ) reaction in 56 Fe releases a prompt gamma ray of Eγ = 7 MeV. a) What is the recoil energy of the 57 Fe product nucleus? b) Determine the number of displaced atoms per 57 Fe recoil assuming Ed = 40 eV. c) If the thermal component of the neutron flux in a fast reactor is 1013 n/cm2 s what is the damage production rate due to the (n,γ ) reaction in 56 Fe?

122

2.7

2.8

2.9

2.10

2.11

2.12

2.13

2 The Displacement of Atoms

d) If the fast flux is given by: φf (En ) = 1015 δ (En − 0.5), where En is in MeV, what is the damage production rate due to the fast flux in iron? Use the K–P displacement formula in (c) and (d). The scattering cross section for 0.5 MeV neutrons is 3 barns. Also, σa56 ∼ 2.5 barns for part (c). Assuming that atom–atom interactions can be treated as near head-on collisions, the appropriate potential function is then the Born–Mayer potential. Write an expression for the threshold energy for unassisted critical focusing along the [110] direction in fcc nickel in terms of the lattice constant, a. For iron (equilibrium phase for 400 ◦C), assuming a focusing collision occurs, how much does the closest approach (the allowed equivalent hard-sphere radius calculated using a Born–Mayer potential) change between a [100] collision chain and a [110] collision chain? a) Calculate the focusing energy of the 111 direction for gold under the condition of assisted focusing. b) Will focusing occur along the 111 direction in the absence of assisted focusing? Why? c) The experimental focusing energy of gold is 21,000 eV for the 111 direction. Compare your answer with this value. a) Determine the critical focusing energy for the 111, 110 and 100 directions in fcc copper and iron. b) Plot θc as a function of T < Ec for the 111 directions in Ni and Fe. Comment on similarities and differences. c) Do the same for the 110 direction of each. d) Repeat parts (a) and (b) using the inverse square potential, V (r) = A/r2 , where A = 1.25 eVnm2 . e) Over what energy range does focused replacement occur? How about focused energy packets only? For the focusing process as described in Problem 2.10, give a physical explanation of why the critical angle for focusing, θc , should depend on the projectile energy. A 30 keV ion enters a channel in the solid lattice and loses energy only by electronic excitation. Using the Lindhard stopping power formula Eq. (1.170), determine the distance traveled by the ion before it is dechanneled. The minimum channeling energy is 300 eV. Use k = 0.003NZ 2/3 eV1/2 /nm, where N is the atomic density of the metal in nm−3 . Show that when channeling is accounted for in the collision cascade, the average number of displaced atoms ν (T ) is:

ν (T ) − (T /2Ed )1−2p , where p is the probability that an atom with energy E being channeled is lost to the cascade. Assume that p = f (E), T Ed , and p 1. Assuming that all energy is lost by elastic collisions for 100 keV protons in nickel determine: a) The energy loss per unit length in the solid, dE/ dx b) The range in the solid.

References

123

2.14 A crystal of copper is bombarded with monoenergetic (2 MeV) neutrons. a) Calculate the mean atomic displacement rate (displacements/cm3 s) using the simple Kinchen–Pease model and the following data: Lattice parameter, Cu = 0.361 nm Atomic weight of Cu = 63.54 amu Displacement energy for Cu = 40 eV φ = 1013 n/cm2 s (2 MeV) σs = 0.5 ×10−24 cm2 (2 MeV) b) Repeat part (a) but instead of 2 MeV neutrons, use a monoenergetic thermal neutron beam where φth = φfast , σth = 3.78×10−24 cm2 and the recoil energy, ER ∼ 382 eV. c) What would be the effect on your answer to part (a) by including Lindhard’s damage energy function ξ (T )? d) How would your answer in part (a) be affected by assuming that the channeling probability is 1%, 5%, 10%? 2.15 For the 2 MeV neutron bombardment problem describe in Problem 2.14, how would you go about calculating the threshold energy for unassisted critical focusing along the [110] direction? 2.16 Assume that the copper target in Problem 2.14 was bombarded by a beam of 2 MeV He ions instead of a beam of 2 MeV neutrons. Calculate the displacement rate at the surface of the sample and compare to your result for Problem 2.14. 2.17 The same copper sample as in Problem 2.14 is bombarded with 500 keV Cu+ ions at a flux of 1015 cm−2 s−1 . Calculate: a) The displacement rate at the surface b) The location of the damage peak. Use a linear interpolation between the values of dE/ dx as given on the attached sheet.

References 1. 2. 3. 4. 5. 6.

7. 8. 9. 10.

Kinchin GH, Pease RS (1955) Rep Prog Phys 17:1 Seitz F (1949) Disc Faraday Soc 5:271 Bacon DJ, Deng HF, Gao F (1993) J Nucl Mater 205:84 King WE, Merkle KL, Meshii M (1983) J Nucl Mater 117:12–25 Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements. US DOE, Washington, DC ASTM E521 (1996) Standard Practice for Neutron Radiation Damage Simulation by Charged-Particle Irradiation. Annual Book of ASTM Standards, vol. 12.02. American Society for Testing and Materials, Philadelphia, PA Robinson MT (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge Snyder WS, Neufeld J (1955) Phys Rev 97(6):1636 Sanders JB (1967) Dissertation, University of Leiden Kohler W, Schilling W (1965) Nukleonik 7:389

124 11. 12. 13. 14. 15. 16.

17. 18. 19. 20. 21.

22. 23. 24. 25.

2 The Displacement of Atoms Sigmund P (1969) Appl Phys Lett 14(3):114 Lindhard J, Nielsen V, Scharff M (1968) Kgl Dan Vidnsk Selsk Mat Fyf Medd 36(10) Sigmund P (1969) Rad Eff 1:15–18 Erginsoy C, Vineyard GH, Englert A (1964) Phys Rev 133A:595 Lindhard J, Nielsen V, Scharff M, Thomsen PV (1963) Dan Vidnsk Selsk Mat Fyf Medd 33:1 Robinson MT (1972) The dependence of radiation effects on the primary recoil energy. In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 397 Norgett MJ, Robinson MT, Torrens IM (1975) Nucl Eng Des 33:50–54 Chadderton LT (1965) Radiation Damage in Crystals. Wiley, New York Brandt W (1968) Sci Amer 218:90 Datz S, Noggle TS, Moak CT (1965) Nucl Instr Meth 38:221 Doran DG (1971) Displacement Cross Sections for Stainless Steel and Tantalum Based on A Lindhard Model, USAEC Report, HEDL-TME-71-42. WADCO Corporation, Hanford Engineering Development Laboratory, April 1971 Robinson MT (1996) J Nucl Mater 216:1–28 Simmons RL, McElroy WN, Blackburn LD (1972) Nucl Technol 16:14 McElroy WN, Dahl RE, Gilbert ER (1970) Nucl Eng Des 14:319 Kulcinski GL, Brimhall JL, Kissinger HE (1972) Production of voids in pure metals by high-energy heavy-ion bombardment. In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 453

3 The Damage Cascade

3.1 Displacement Mean Free Path In our discussion of cascade development, no consideration was given to the spatial arrangement of displaced atoms. We assumed that every Frenkel pair created was preserved and that no annihilation occurred. However, the spatial arrangement of these Frenkel pairs is crucial in determining the number that survive annihilation or immobilization by clustering. In order to understand what the damaged region looks like, we need to know if the displacements are concentrated or distributed. A helpful tool in this regard is the mean free path for displacement collisions, i.e., collisions in which the energy transferred is greater than Ed . This will tell us how far apart the displacements occur and hence, the separation distance between Frenkel pairs. 1 By definition, the mean free path, λ = and the corresponding displacement Nσ cross section is:

σd (E) =

E Ed

σ (E, T ) dT .

(3.1)

This is the cross section for the transfer of energy in excess of Ed and is given in terms of the differential energy transfer cross section between lattice atoms. Note that σd has nothing to do with the projectile, be it a neutron or an ion, or the source of the damage in general. Using the equivalent hard-sphere model to evaluate σd gives:

σ (E) , γE but γ = 1, so substituting into Eq. (3.1) and integrating yields: E Ed σ (E) dT = σ (E) 1 − σd (E) = , E E Ed σ (E, T ) =

(3.2)

where σ (E) = 4π r2 is the total collision cross section between lattice atoms, so: Ed , (3.3) σd (E) = 4π r2 1 − E and r is the energy-dependent, equivalent hard-sphere radius, which, using the Born–Mayer potential gives:

2 2A Ed 2 σd (E) = π B ln 1− , (3.4) E E

126

3 The Damage Cascade

and the mean free path, λ becomes:

λ=

1 .

2 2A Ed 2 1− N π B ln E E

(3.5)

The mean free path and the total collision cross section are plotted in Fig. 3.1 for copper atoms in copper, and show that as the energy of the moving atom drops, the cross section increases slowly but the mean free path becomes very small at energies just above Ed . Note that the critical region (λ ∼ 0.3 – 1.0 nm), or the region in which every lattice atom in the path of the knock-on is displaced, lies in the energy range ∼ 50 – 100 eV. The mean free paths for primary recoil atoms of 300 keV and 1 MeV resulting from self-ion irradiations of Si, Cu and Au are shown in Fig. 3.2. Recall that T¯ = γ Ei ∼ 2Ei (for n-Cu interactions), where Ei is the neutron energy and A is the = 2 A atomic mass. Typically, Ei ∼ 0.5 MeV (for a thermal or fast reactor) and A ∼ 60 (stainless steel), giving T¯ ∼ 15 keV. So at large recoil energies, the displacements are well separated (∼ 100 nm at 15 keV), but as the recoil energy decreases, the spacing approaches the atomic spacing, at which point each atom along the recoil path is displaced.

3.2 Primary Recoil Spectrum The analysis of displacement mean free path gives us a first glimpse of what the spatial distribution of defects might look like. Brinkman [3] was the first to picture the cascade as a displacement spike with a high core density of vacancies surrounded by an interstitial shell (Fig. 3.3). Seeger [4] modified the picture to account for crystallinity such as focused energy packets (focusons), and long-range transport of mass by replacement collisions and channeling, and termed the vacancy core a depleted zone (Fig. 3.4). Two additional quantities are helpful in developing a picture of the distribution of damage energy. The first is the deposited energy depth distribution, FD (x), defined by: FD (x) dx = dE = NSn E(x) dx .

(3.6)

Using the nuclear stopping power and range given by the power law potential [5] results in a simple form for FD (x): FD (x) =

1 T (1 − x/R) 2m −1 , 2mR

(3.7)

where T is the PKA energy, R is the PKA range and m = 1/s where s is the power law exponent. If Nd (x) is the number of displacements per unit depth at a depth x, then using the modified K–P model or the NRT model (e.g., Eq. (2.53)) with κ = 0.8

3.2 Primary Recoil Spectrum

127

Fig. 3.1. Displacement mean free path and total collision cross section for copper atoms moving in copper (after [1])

Fig. 3.2. Mean free paths of primary recoil atoms of 300 keV and 1 MeV, self-ion irradiations of Si, Cu and Au (after [2])

128

3 The Damage Cascade

Fig. 3.3. Original version of the displacement spike as drawn by Brinkman (after [3])

Fig. 3.4. Revised version of Brinkman’s displacement spike as drawn by Seger (after [4]) accounting for crystallinity in the damage cascade

and with FD (x) replacing ED , we can write that: Nd (x) 0.8FD (x) = , φ 2Ed

(3.8)

and the displacement rate as a function of depth in units of dpa becomes: dpa(x) =

Nd (x) 0.4FD (x) = φ. N NEd

(3.9)

3.2 Primary Recoil Spectrum

129

The total dpa produced over the range of the recoil can be estimated by replacing FD (x) with the damage energy ED from Eq. (2.54) over the range of the recoil, R: dpa ∼ =

φ 0.4ED . NREd

(3.10)

The second important concept is the primary recoil spectrum. The density of recoil atoms with energies between T and T + dT that occur during irradiation is an important quantity in radiation damage. The recoil density depends on the projectile energy and mass and gives a measure of the density of displacement damage in the target. The density of recoils as a function of recoil energy is known as the primary recoil spectrum and is given as: P(Ei , T ) =

1 N

T Ed

σ (Ei , T ) dT ,

(3.11)

which is the fractional number of recoils between the minimum displacement energy Ed , and energy T , and N is the total number of primary recoils, and σ (Ei , T ) is the energy transfer cross section for a particle of energy Ei to create a recoil of energy T . The fraction of recoils is shown in Fig. 3.5 for 1 MeV projectiles of various mass incident on a copper target. Note that while higher mass projectiles produce more recoils at higher energy, the difference does not appear to be large. For defect production, it is not the number of recoils of a particular energy that is of greatest importance, rather it is the fraction of damage energy that are produced

Fig. 3.5. Integral primary recoil spectra for 1 MeV particles in copper. Curves plotted are the integral fractions of primary recoils between the threshold energy and energy, T from Eq. (3.11) (after [2])

130

3 The Damage Cascade

in recoils of a particular energy. This quantity is given by “weighting” the recoil spectra by the number of defects or the damage energy produced in each recoil: W (Ei , T ) =

1 ED (Ei )

T Ed

σ (Ei , T )ED (T ) dT ,

(3.12)

where ED (T ) is the damage energy created by a recoil of energy T : ED (Ei ) =

Tˆ Ec

σ (Ei , T )ED (T ) dT ,

(3.13)

and Tˆ = γ Ei . For the extremes of Coulomb and hard-sphere interactions, the differential energy-transfer cross sections are:

σCoul (Ei , T ) =

π M1 (Z1 Z2 ε 2 )2 , Ei T 2

(3.14)

and

σHS (Ei , T ) =

A . Ei

(3.15)

Ignoring electron excitations and allowing ED (T ) = T , and substituting Eqs. (3.14) and (3.15) into Eq. (3.12) gives the weighted average recoil spectra for each type of interaction: WCoul (T ) =

ln T − ln Tˇ , ln Tˆ − ln Tˇ

(3.16)

and WHS (T ) =

2 T 2 − Tˇ Tˆ 2

(3.17)

where Tˇ = Ed . Equations (3.16) and (3.17) are graphed in Fig. 3.6 for 1 MeV particle irradiations of copper. The Coulomb potential is a good approximation for proton irradiation while the hard-sphere potential is a good approximation for neutron irradiation. The Coulomb forces extend to infinity and slowly increase as the particle approaches the target. In a hard-sphere interaction, the particles and target do not “feel” each other until their separation reaches the hard-sphere radius at which point the repulsive force goes to infinity. A screened Coulomb is most appropriate for heavy ion irradiation. The result is that Coulomb interactions tend to create many PKAs with low energy while hard-sphere collisions create fewer PKAs but with higher energy. Note the large difference in W (T ) between the various types of irradiations in Fig. 3.6. While heavy ions come closer to reproducing the energy distribution of recoils of neutrons than do light ions, neither is accurate in the “tails” of the distribution. This does not mean that ions are poor simulations of radiation

3.3 Cascade Damage Energy and Cascade Volume

131

Fig. 3.6. Weighted recoil spectra for 1 MeV particles in copper, (after [2]). Curves representing protons and neutrons are calculated using Eqs. (3.14) and (3.15), respectively. W (T ) for other particles were calculated using Lindhard cross sections and include electronic excitation

damage, but it does mean that damage is produced differently and that this needs to be considered when assessing the microchemical and microstructural changes due to irradiation. Figure 3.7 illustrates the difference in the types of damage that is produced by different types of particles. Light ions such as electrons and protons will produce damage as isolated Frenkel pairs or in small clusters while heavy ions and neutrons produce damage in large clusters. For 1 MeV particle irradiation of nickel, half the recoils for protons are produced with energies less than ∼ 1 keV but with an average energy of 60 eV while the same number for Kr occurs at about 30 keV with an average energy of 5 keV. Recoils are weighted toward lower energies because of the screened Coulomb potential that controls the interactions of charged particles. For an unscreened Coulomb interaction, the probability of creating a recoil of energy T varies as 1/T 2 . Because neutrons interact as hard spheres, the probability of a creating a recoil of energy T is independent of recoil energy.

3.3 Cascade Damage Energy and Cascade Volume The energy density in a cascade of volume Vcas formed by an energetic projectile of energy Ei is given by [7]: ED Θ¯ D ∼ , = NVcas

(3.18)

132

3 The Damage Cascade

Fig. 3.7. Difference in damage morphology, displacement efficiency and average recoil energy for 1 MeV particles of different type incident on nickel (after [6])

where ED is the damage energy defined in Eq. (2.54) and N is the atom density of the target. To find the volume of the cascade requires knowledge of the depth distribution of the damage energy. Averback [2] showed that the volume of the cascade can be approximated by: Vcas =

4π ((δ ΔX)2 + 2(δ Y )2 )3/2 , 3

(3.19)

where (ΔX)2 and Y 2 are the longitudinal and transverse moments of the deposited damage energy distribution for an individual cascade, and δ is a contraction factor that accounts for the difference between an individual cascade and the average cascade determined by transport theory. While Eqs. (3.18) and (3.19) provide a description of the spatial extent of a cascade, other characteristics of the cascade are the temperature and temporal lifetime. The effective temperature of the cascade can be estimated by the relation: 3kB Tmax = Θ¯ D ,

(3.20)

where kB is Boltmann’s constant. The lifetime of the cascade or thermal spike can be estimated by solving the heat equation for the spread of energy from a point source in three dimensions. The variance in the temperature profile, R2 , is given by: R2 = 4Dτ ,

(3.21)

3.4 Computer Simulations of Radiation Damage

133

where τ is the cascade lifetime and D is the thermal diffusivity = κT /Cp , where κT is the thermal conductivity and Cp is the specific heat capacity. The cascade energy is then: 4 ED = π R3Ua N , 3

(3.22)

where Ua is the energy per atom. The cascade lifetime is determined by combining Eqs. (3.21) and (3.22) to solve for τ : 3ED 1 τ= . (3.23) 4D 4π NUa If we estimate Ua from the melting temperature of the target, then Ua ∼ 0.3 eV and D ∼ 1012 nm2 /s, then the lifetime of a 1 keV cascade is of the order 10−12 s, or a few lattice vibration periods.

3.4 Computer Simulations of Radiation Damage Analytical solutions to the space and time dependence of damage caused by an energetic particle incident on a target can take us only so far. And as we will see later, excellent instrumentation exists to observe defect clusters such as transmission electron microscopy, X-ray scattering, small angle neutron scattering and positron annihilation spectroscopy. But these instruments do not have the resolution to image individual defects and they cannot capture the temporal development of the cascade. To gain a better understanding of the spatial and temporal development of the cascade, we must turn to computer simulation. There are three principal techniques used to model the behavior of atoms in a displacement cascade; the binary collision approximation (BCA) method, the molecular dynamics (MD) method and the kinetic Monte Carlo (KMC) method [8]. Each will be briefly discussed. 3.4.1 Binary Collision Approximation (BCA) Method BCA simulations are useful for examining the collisional stages of high-energy cascades in statistically significant numbers. BCA simulations consider only the interactions between two colliding atoms at a time and in sequence [8]. The computation follows only the atoms having significant energies and are thus very efficient. The BCA approach provides a good approximation to the collision stage, since the neglected many-body interactions make little contribution to the atom trajectories at collision energies well above the atom displacement energy. At energies near or even less than the displacement energy, ballistic features of cascades such as replacement-collision sequences and focused-collision sequences (focusons) can be reasonably captured by BCA calculations. At primary recoil energies above approximately 20 keV, cascades may have more than one damage region. Because the mean free path between high-energy collisions of a recoil atom increases with energy,

134

3 The Damage Cascade

higher energy cascades will consist of multiple damage regions or subcascades that are well separated in space due to high-energy collisions. Channeling of primary or high-energy secondary recoils also contributes to subcascade formation when the channeled recoils lose energy and de-channel. There are two distinct types of BCA models. Those for crystalline targets are termed BC or binary crystal models and resemble MD models in that they assign all atoms to well-defined initial positions [9]. Models for materials without longrange order (amorphous solids) are termed MC or Monte Carlo models and use stochastic methods to locate target atoms and to determine collision parameters. The MC models are similar to transport theory models used in analytical theory to track neutron populations in a medium. An example of a BC model is the MARLOW code [10]. The program models crystalline targets with no restrictions on the crystal symmetry or on the chemical composition. All collision parameters are calculated from the particle positions. Several interatomic potentials are available for selection to describe atom collisions. Inelastic energy losses may be included in either local or non-local form, but the loses are limited to the velocity-proportional (E 1/2 ) range of kinetic energies. Figure 3.8 shows the spatial configuration of defects from an early computer simulation using the MARLOWE code for the case of a 200 keV cascade in copper. This is a very energetic cascade that would only be expected from extremely energetic neutrons such as are generated in a fusion reactor. The PKA is generated in the lower

Fig. 3.8. Collisional stage of a 200 keV cascade in copper simulated using the binary collision approximation in MARLOWE (after [8])

3.4 Computer Simulations of Radiation Damage

135

Fig. 3.9. Computer simulation of a displacement spike due to a 5 keV PKA in iron. All out-ofplane damage has been projected onto the 001 plane shown in the figure. (a) Recoil trajectories and (b) vacancies and interstitial atoms at the end of the collision cascade (0 K). The diagonal line in (b) shows the effect of channeling of a secondary knockon atom (after [11])

right hand corner (arrow) and proceeds to the left with a kinetic energy of 200 keV. The dark spheres are displaced atoms and the lighter spheres are vacant lattice sites. Note that the full cascade consists of several subcascades. A second example, shown in Fig. 3.9 shows how the cascade can become extended in space. The recoil trajectories and final configuration of interstitials and vacancies in bcc iron is shown after interaction with a 5 keV PKA at a temperature of 0 K [11]. All vacancies and interstitials within a sphere containing 30 lattice atom sites were assumed to recombine spontaneously. Note in Fig. 3.9a, that the secondary knock-on in the center of the spike undergoes channeling, making possible the extension of the cascade into the upper right half of the lattice shown in Fig. 3.9b. Essentially, all of the damage to the upper right of the diagonal is due to channeling of the secondary knock-on.

136

3 The Damage Cascade

TRIM [12] is another BCA code that uses Monte Carlo techniques to describe the trajectory of the incident particle and the damage created by that particle in amorphous solids and was discussed briefly in Chap. 1. TRIM uses a maximum impact parameter set by the density of the medium and a constant mean free path between collisions which is related to this. Stochastic methods are used to select the impact parameter for each collision and to determine the scattering plane. The barycentric scattering angle is determined by a “magic” formula, tested against published integral tables and represents the scattering from the ZBL “universal” potential. Inelastic energy losses are based on the effective charge formalism, using tables distributed with the code. Figure 3.10 shows a simulation of 3 MeV protons incident on a nickel target. Figure 3.10a shows the trajectories of the incident particles for 10,000 cases (MC runs), and Fig. 3.10b shows the ion concentration profile and the displacement rate profile as a function of depth. 3.4.2 Molecular Dynamics (MD) Method Molecular dynamics is the second major type of methodology used to describe collision cascades. MD is a computationally intensive method for modeling atomic systems on the appropriate scale for the simulation of displacement cascades and provides the most realistic description of atomic interactions in cascades [8]. Using realistic interatomic potentials and appropriate boundary conditions, the fate of all atoms in a volume containing the cascade can be described through the various stages of cascade development. The analytical interatomic potential functions must describe the force on an atom as a function of the distance between it and the other atoms in the system. It must account for both attractive and repulsive forces in order to obtain stable lattice configurations. In MD simulations, the total energy of the system of atoms being simulated is calculated by summing over all the atoms. The forces on the atoms are used to calculate acceleration according to F = ma, yielding the equations of motions for the atoms. The computer code solves these equations numerically over very small time steps, and then recalculates the forces at the end of the time step, to be applied in the calculations in the next time step. The process is repeated until the desired state is achieved. Time steps in MD simulation must be very small (5 – 10 ×10−15 s), so MD simulations are generally run for no more than 100 ps. As the initial primary kinetic energy E increases, larger and larger numerical crystallites are required to contain the event. The size of the crystallite is roughly proportional to E. The required computing time-scales roughly as E 2 . The demand on computing time limits the statistical capabilities of MD simulation. However, they provide a detailed view of the spatial extent of the damage process on an atomic level that is not afforded by other techniques. A cascade simulation begins by thermally equilibrating a block of atoms that constitutes the system to be studied. This process allows the determination of the lattice vibrations for the simulated temperature. Next, the cascade simulation is initiated by giving one of the atoms a specified amount of kinetic energy and an initial direction. Several cascades must be run in order to have results that can

3.4 Computer Simulations of Radiation Damage

137

Fig. 3.10. A 3 MeV proton incident on nickel as modeled by the TRIM code: (a) trajectory, (b) concentration profile and displacement profile

be used to represent the average behavior of the system at any energy and temperature. One such code used for MD simulations is the MOLDY code written by Finnis [13] and uses interatomic potentials developed by Finnis and Sinclair [13], and later modified by Calder and Bacon for cascade simulations [14]. The code only describes elastic collisions between atoms, and does not account for energy loss mechanisms such as electronic excitation and ionization. The energy given

138

3 The Damage Cascade

to the PKA in the MD simulation is that corresponding to the value of the displacement energy ED , given in Eq. (2.54). Stoller [15] conducted an MD simulation for iron and generated the cascade parameters shown in Table 3.1. Note that with increasing energy, the difference between the MD cascade energy and the PKA energy increases. Figure 3.11 shows typical point defect configurations from a 1 keV MD cascade simulation in iron at 100 K. Figure 3.11a shows the cascade at the point of peak disorder and Fig. 3.11b shows the cascade following in-cascade recombination. Note the sizable reduction in the residual damage between 0.18 ps and 9.5 ps. This result shows that the actual damage resulting from the PKA is much less than the total aggregate number of displacements calculated from the K–P or NRT models. While “still” images of the stages of the cascade are useful in understanding how the cascade develops, a much better appreciation is gained by viewing the temporal evolution of the cascade directly. This can be done by viewing Movie 3.1 via the website at www.sitemaker.umich.edu/was. This MD simulation shows the development of a cascade from a 200 keV recoil in iron at 100 K through to cascade quench at 21.6 ps. Note the extension of the cascade to the lower right hand corner that is probably do to a crystallographic effect involving channeling. Also note the striking difference in the defect density between the peak ballistic stage (∼ 0.7 ps) and the end of the quench at 21.6 ps.

3.4.3 Kinetic Monte Carlo (KMC) Method Our objective is to simulate the dynamical evolution of systems of atoms during and immediately following the displacement event. The most robust tool in this class of atomistic simulation methods is molecular dynamics. Integrating the classical equations of motion forward in time, the behavior of the system emerges naturally, requiring no intuition or further input from the user. A serious limitation, however, is that accurate integration requires time steps short enough (∼ 10−15 s) to resolve the atomic vibrations. Consequently, the total simulation time is typically limited to less than one nanosecond, while processes we wish to study (e.g., diffusion and annihilation of defects after a cascade event) often take place on much longer timescales. This is the “time-scale problem”. Kinetic Monte Carlo attempts to overcome this limitation by exploiting the fact that the long-time dynamics of this kind of system typically consists of diffusive jumps from state to state. Rather than following the trajectory through every vibrational period, these state-to-state transitions are treated directly. Given a set of rate constants connecting states of a system, KMC offers a way to propagate dynamically correct trajectories through the state space. If the rate catalog is constructed properly, the easily implemented KMC dynamics can give exact state-to-state evolution of the system, in the sense that it will be statistically indistinguishable from a long molecular dynamics simulation. KMC is the most powerful approach available for making dynamical predictions at the mesoscale without resorting to more dubious model assumptions. It can also be used to provide input to and/or verification for higher-level treatments such as rate theory models

3.4 Computer Simulations of Radiation Damage

139

Fig. 3.11. Typical point defect configurations from a 1 keV MD simulation in iron at 100 K at (a) the time of peak disorder (0.18 ps) and (b) following in-cascade recombination (9.5 ps). The larger, lighter spheres are interstitials, and the smaller, darker spheres are vacancies (after [15])

Table 3.1. Typical MD cascade parameters and required atom block sizes (from [15]) Cascade energy EMD ∼ ED (keV)

Corresponding PKA energy (keV)

NRT defects (NRT )

Atom block size (atoms)

0.1 0.2 0.5 1.0 2.0 5.0 10.0 20.0 50.0

0.116 0.236 0.605 1.24 2.54 6.61 13.7 28.8 61.3

1 2 5 10 20 50 100 200 400

3456 6750 6750 54,000 54,000 128,000 250,000 250,000 1,024,000

140

3 The Damage Cascade

Fig. 3.12. Time-scale for radiation damage evolution and the corresponding simulation methodologies

or finite-element simulations. Moreover, even in situations where a more accurate simulation would be feasible (e.g., using accelerated molecular dynamics or on-thefly kinetic Monte Carlo), the extreme efficiency of KMC makes it ideal for rapid scans over different conditions, for example, and for model studies. The result is that KMC can reach vastly longer time-scales, typically seconds and often well beyond. An example of the capability of KMC to capture processes on a larger timescale is given in Movie 3.2, which shows a KMC simulation of a 20 keV cascade in Fe–0.2Cu–0.6Si–0.7Ni–12.4Mn (similar to a pressure vessel steel) at 327 ◦C. The simulation shows the enrichment of Ni (green), Mn (black), Si (blue) and Cu (red) at cascade debris (vacancies in yellow) covering a time period out to several years, or many orders of magnitude longer than the cascade quench time. Note the pairing of Ni and Si and the accumulation of solute atoms at the vacancy clusters. Taken together, the MD and KMC methods cover the radiation time-scale as shown in Fig. 3.12. MD simulations are practical up to the ns range, and KMC simulations extend the range to the second [s] regime. Much occurs after this timescale and this is generally modeled using rate theory, which will be discussed in Chap. 5 and beyond.

3.5 Stages of Cascade Development The final state of the cascade is extremely important because the end of the cascade is the starting point for defect diffusion, agglomeration and destruction that forms the basis for the observable effects of irradiation to be covered in Part II of this text. Figure 3.13 shows another example in which a 2D cross section of a cascade is shown at times that correspond to the early stages of the cascade and near the final state. Here again, the damage state has relaxed to a very large degree between 2 ps (Fig. 3.13a) and 18 ps (Fig. 3.13b). Figure 3.14 shows the radial pair correlation function for the two times. The pair correlation function describes the separation of atoms and will appear as a series of spikes for crystalline solids (by virtue of their long-range order) and as a smoothly varying function for a liquid or amorphous solid (in which there is only nearest and second nearest neighbor correlation). As shown in the figure, the atom arrangement in the core of the displace-

3.5 Stages of Cascade Development

141

Fig. 3.13. MD simulation of a 30 keV displacement cascade in Cu at 300 K at 2 ps and 18 ps into the collision (calculations performed at the Barcelona Supercomputer center, courtesy of M. Catula and Tomas Diaz de la Rubia)

142

3 The Damage Cascade

Fig. 3.14. Pair correlation function for the collision cascades in Fig. 3.13, showing the amorphous-like character of the displacement cascade zone at 2 ps and the considerable degree of recovery by 18 ps (calculations performed at the Barcelona Supercomputer center, courtesy of M. Catula and Tomas Diaz de la Rubia)

ment spike at short times is similar to that of a liquid, while the final arrangement is recovering its crystalline configuration. Figure 3.15 shows that the mean square atomic displacement of atoms in the cascade also increases dramatically with time, indicating that the bulk of the aggregate movement of atoms in the displacement cascade occurs after the time to reach peak damage! Taken together, the results of Figs. 3.13–3.15 tell us that damage is annealing out with time. This annealing is occurring as the energy of the cascade is dropping. In fact, annealing occurs at the tail end of the period during which the cascade energy drops, called the quench stage. We now have a picture of how the cascade develops in time that we can describe. Cascades evolve in stages given as follows: 1. 2. 3. 4.

Collisional Thermal spike Quenching Annealing

In the collisional stage (1), the primary recoil atom initiates a cascade of displacive collisions that continues until no atom contains enough energy to create further displacements. At the end of this stage (lasting < 1 ps), the damage consists of energetic displaced atoms and vacant lattice sites. However, stable lattice defects have

3.6 Behavior of Defects within the Cascade

143

Fig. 3.15. Integrated diffusion coefficient as a function of distance from the center of the cascade at the end of the collisional phase, t = 0.12 ps (solid diamonds) and at the end of the cooling phase, t = 10 ps (open squares), for a 5 keV cascade in copper (after [16])

not yet had time to form. During the thermal spike stage (2), the collisional energy of the displaced atoms is shared among their neighboring atoms in the region of high deposited energy density. The development of the spike requires about 0.1 ps, and the spike may occupy several zones in which the energy is high enough so that the atoms resemble molten material. As energy is transferred to the surrounding atoms, the molten zones return to the condensed, or quenched stage (3), and thermodynamic equilibrium is established (∼ 10 ps). The quenching stage may take several ps and during this time, stable lattice defects form either as point defects or as defect clusters. But the total number of defects at this stage is much less than the number of atoms displaced in the collisional stage. The annealing stage involves further rearrangement and interaction of defects and occurs by thermally activated diffusion of mobile lattice defects. By definition, the annealing stage (4) lasts until all mobile defects escape the cascade region or another cascade occurs within it. Thus, the timescale extends from nanoseconds to months, depending on the temperature and the irradiation conditions. The annealing stage is the subject of the next part on Physical Effects of Radiation Damage (Part II) and is the link between the damage cascade and the observable effects of irradiation.

3.6 Behavior of Defects within the Cascade The actual number of defects that survive the displacement cascade and their spatial distribution in the solid will determine their effect on the irradiated microstructure. We define the displacement efficiency ξ , as the fraction of the “ballistically” produced Frenkel pairs (NRT dpa) that survive the cascade quench. MD simulation of the displacement cascade provides the recoil dependence of the displacement effi-

144

3 The Damage Cascade

Fig. 3.16. Dependence of the displacement efficiency on median PKA in copper. Open symbols refer to MD calculations and filled symbols refer to experimental measurements as the result of electron (•), ion (), fission fragment () and neutron () irradiation at low temperatures (after [17])

ciency in copper irradiated at low temperature (Fig. 3.16). The value of ξ increases rapidly from zero to > 1 at very low recoil energies. That ξ exceeds 1.0 is attributed to the inability of the modified K–P model to describe displacements in a polycrystalline material at recoil energies near the threshold displacement energy, Ed , due to the strong dependence of Ed on crystallographic orientation [17]. With increasing energy, ξ steadily decreases to a value of about 0.3 for 5 keV cascades in copper. The formation of multiple subcascades at high PKA energies (above ∼ 20 keV) causes ξ to remain nearly constant for PKA energies up to 500 keV. Comparing this plot to the recoil and weighted recoil spectra given in Figs. 3.5 and 3.6 shows that electrons and light ions with a low PKA energy will generate values of ξ close to 1, while heavy ions and neutrons that produce high PKA energies will result in ξ at the asymptotic value of 0.3. The displacement cascade efficiency, ξ is comprised of several components:

γi,v The isolated point defect fraction δi,v Clustered fraction including mobile defect clusters such as di-interstitials ζ Fraction initially in isolated or clustered form after the cascade quench that is annihilated during subsequent short term (> 10−11 s) intracascade thermal diffusion They are related as follows:

ξ = δi + γi + ζ = δv + γv + ζ .

(3.24)

3.6 Behavior of Defects within the Cascade

145

Fig. 3.17. Interdependence of isolated point defects, mobile defect clusters, and thermally evaporating defect clusters that contribute to the fraction of surviving defects that are “available” for radiation effects (after [17])

Figure 3.17 shows the history of defects born according to the NRT model as vacancies and interstitials. The fraction of defects that will be annihilated after the cascade quench by recombination events among defect clusters and point defects within the same cascade (intracascade recombination), ζ is about 0.07, for a displacement efficiency of 0.3. The clustered fraction, δ includes large, sessile clusters and small defect clusters that may be mobile at a given irradiation temperature and will be different for vacancies and interstitials. For a 5 keV cascade, δi is about 0.06 and δv is closer to 0.18. Some of these defects may be able to “evaporate” or escape the cluster and become “available” defects (Fig. 3.17). This leaves γ , the isolated point defect fraction as yet to be determined. These defects are available to migrate to sinks, to form clusters, to interact with existing clusters and to participate in the defect flow to grain boundaries that gives rise to radiation-induced segregation. Because of their potential to so strongly influence the irradiated microstructure, defects in this category, along with defects freed from clusters, make up the freely migrating defects (FMD). Recall that electrons and light ions produce a large fraction of their defects as isolated Frenkel pairs, thus increasing the likelihood that they remain as isolated defects rather than in clusters. Despite the equivalence in energy among the four particle types described in Fig. 3.7, the

146

3 The Damage Cascade

average energy transferred and the defect production efficiencies vary by almost two orders of magnitude! This is explained by the differences in the cascade morphology among the different particle types. Neutrons and heavy ions produce dense cascades that result in substantial recombination during the cooling or quenching phase. However, electrons are just capable of producing a few widely spaced Frenkel pairs (FP) that have a low probability of recombination. Protons produce small widely spaced cascades and many isolated FPs due to the Coulomb interaction and therefore, fall between the extremes in displacement efficiency defined by electrons and neutrons. The value of γ has been estimated to range from 0.01 to 0.10 depending on PKA energy and irradiation temperature, with higher temperatures resulting in the lower values. Because of the importance of this parameter, we will estimate the freely migrating defect fraction using an analytical treatment by Naundorf [18] that is based on two factors. The first is that energy transfer to atoms is only sufficient to create a single Frenkel pair. The second is that the Frenkel pair lies outside a recombination (interaction) radius so that the nearby FPs neither recombine nor cluster. The model follows each generation of the collision and calculates the fraction of all defects produced that remain free. According to Naundorf, the free single FPs are classified according to the generation i in which they were produced, i.e., the relative amount η1 is that amount that is produced by primary collisions (first generation), while η2 is the relative amount produced by secondary collisions (second generation). Thus the total number of free single FPs produced is:

η = ∑ ηi ,

(3.25)

i

where that produced by primary collisions is:

η1 = (βp /σd )

γE Ed

σ (Ei , T ) dT ,

(3.26)

and that produced by secondary collisions is:

η2 = (1/σd )

γE Ed

σ (Ei , T )[Z(T )βA (T )/σA (T )] dT

2.5Ed Ed

σ (T, T ) dT , (3.27)

where σ (Ei , T ) is the energy transfer cross section for an incident particle to a lattice atom and σ (T, T ) is the energy transfer cross section between like atoms in the solid, Z(T ) is the total number of secondary collisions produced above Ed by a PKA of energy T along its path. The primary displacement cross section for the incident ion, σp , is:

σp =

γE Ed

σ (Ei , T ) dT ,

(3.28)

and the total displacement cross section σd is given in the Kinchin–Pease model by:

σd =

γE Ed

σ (Ei , T )ν (T ) dT .

(3.29)

3.6 Behavior of Defects within the Cascade

147

The distance λ between two primary collisions is distributed according to an exponential law: W (λ ) = 1/λp exp(−λ /λp) ,

(3.30)

with the mean distance:

λp = Ω /σp ,

(3.31)

where Ω is the atomic volume. The condition that the distance between two consecutive collisions must be larger than an appropriate interaction radius, ri (so that FPs produced near each other neither recombine nor cluster) reduces the amount of all possible free single FPs by:

βp = exp(−ri /λp ) ,

(3.32)

and is illustrated in Fig. 3.18 [19]. The model provides the efficiency for the production of freely migrating defects. Results of this calculation are shown in Table 3.2 for several ions of varying mass and energy. Values of η range between 24% for proton irradiation to 3% for heavy ion (krypton) irradiation. Applying this model to our illustration in Fig. 3.7 yields the following values for η : MeV electrons: 3.4 MeV protons: 5.0 MeV Ni++ ions: Neutrons (fission spectrum):

1.0 0.2 0.04 0.02

These results can also be compared to those calculated by Rehn et al. [20] determined from analysis of experiments and are shown in Fig. 3.19. The data in this

Fig. 3.18. Illustration of the effect of the interaction radius on single Frenkel pair production

148

3 The Damage Cascade

Table 3.2. Calculated values for σp /σd and of the relative amounts ηcalc of FP production in nickel by different kinds of irradiations (Ed = 40 eV, ri = 0.7 nm) using Lindhard’s analytical differential collision cross section (from [18]) Irradiation

σp /σd (%)

ηcalc (%)

1 MeV H+ 2 MeV H+ 2 MeV Li+ 1.8 MeV Ne+ 300 keV Ni+ 3 MeV Ni+ 3.5 MeV Kr+ 2 keV O+

37.0 30.0 27.0 16.0 5.1 7.5 5.9 42.0

24.0 19.2 16.9 8.7 2.3 3.8 3.0 9.8

Fig. 3.19. Relative efficiency of freely migrating defect production for ions of various mass and energy (after [20])

figure are arbitrarily normalized to 1.0 for 1 MeV protons. This data along with the results just presented show that at low recoil energies, the fraction of defects that are freely migrating approaches 1.0 and as the recoil energy increases, that fraction drops to values in the range 0.02 to 0.05. Recent results [21], however, have shown that the low values of FMD efficiency for heavy ion or neutron irradiation cannot be explained by defect annihilation within the parent cascade (intracascade annihilation). In fact, cascade damage generates vacancy and interstitial clusters that act as annihilation sites for FMD,

3.6 Behavior of Defects within the Cascade

149

reducing the efficiency of FMD production. Thus, the cascade remnants result in an increase in the sink strength for point defects and along with recombination in the original cascade, account for the low FMD efficiency measured by experiment. While the NRT description of atom displacements provides an estimation of the number of Frenkel pairs produced by the PKA, it does not accurately describe atomic interactions in the thermal spike and hence, is inadequate for describing the true configuration of defects. MD simulations can be used for this purpose and have confirmed that defect production by displacement cascades is not as efficient as predicted by the NRT formula. In fact, ν is about 20 to 40% of NRT for cascades with energy greater than 1 – 2 keV. From analysis of MD results for several metals [22], the number of Frenkel pairs is found to depend on the kinetic energy of the PKA, T as:

νMD = AT n ,

(3.33)

where A and n are constants that are only weakly dependent on the metal and temperature. Figure 3.20 shows the dependence of νMD on T for various metals. Note that the behavior of Frenkel pair production is well represented by this function over a large damage energy range. Also note that the results all fall below the NRT value as shown by the solid line in the figure. The lower efficiency is likely the result of SIA production at the periphery of the disordered core dominating that at the end of focused collision chains such that the close proximity to the vacancies and the high kinetic energy of the core during the thermal spike assist in SIA-vacancy recombination. From the results shown in Fig. 3.20, there is no noticeable dependence on the crystal structure, as there are three fcc metals (Al, Ni, Cu), two hcp metals (Ti, Zr), one bcc metal (Fe) and one ordered L12 structure (Ni3 Al), and yet the magnitude of νFP is not separated along crystal structure lines. Second, there is a dependence on atomic mass of the metal as noted in the dependence of νMD and A on T . The dependence of n on atomic mass is weaker, though evident. The decrease in efficiency with atomic mass is likely due to the enhanced recombination due to thermal spike effects. As cascade energy increases, there is a tendency for cascades to break up into subcascades. Since one cascade produces fewer defects than two separate cascades of the same total energy, subcascade formation will increase the slope of the plots in Fig. 3.20. The transition to subcascades occurs at lower energy in lighter metals and may be the cause for the mass-dependence on efficiency. Note that n is only weakly dependent on mass. MD simulation has also been applied to the study of defect production in alloys [23, 24]. One might expect that the mass difference between solute atoms in an alloy will interrupt crystallographic processes such as focusing and channeling and result in the production of more Frenkel pairs as compared to the pure metal case. MD simulations in copper containing up to 15 at% gold in solution shows that the larger Au atoms decrease the length of focused displacement events in the ballistic phase and thereby enhance the intensity and lifetime of the disorder and temperature of the thermal spike. However, νFP was found to be independent on

150

3 The Damage Cascade

the alloy composition over a wide range of T . Similar studies conducted on Fe–Cu alloys substantiated these results. Movie 3.3 shows cascade formation and cooling in an Fe–10%Cr alloy in which the yellow balls are vacancies, the grey are iron interstitials and the green are chromium interstitials. In this simulation chromium is modeled as the larger solute, and after cooling, the remaining interstitial population is predominantly iron atoms as their distortion of the lattice is less than that from the oversized chromium atoms. The results shown in Fig. 3.20 are for MD calculations at or below a temperature of 100 K. Irradiation temperature has a strong effect on the evolution of radiation damage in metals because of its effect on the motion of defects and their stability as clusters. Irradiation temperature also has an effect on the formation of Frenkel pairs. Figure 3.21 shows the Frenkel pair production as a function of temperature in α -iron up through 900 K (627 ◦C) and for several values of PKA energy. Note that there is a small but consistent effect of temperature in that higher irradiation temperatures produce fewer Frenkel pairs. The lower Frenkel pair production is believed to be due to the increase in the lifetime of the thermal spike as Tirr increases, which allows for more defect motion before cooling and hence, more vacancy-interstitial recombination within the cascade region. A contributing factor may be the shorter length of the focused collision sequences (due to the higher kinetic energy of the atoms) that results in a reduction of the vacancy-interstitial separation distance.

Fig. 3.20. Number of Frenkel pairs produced as a function of damage energy, T for Cu, Fe, Ti, Zr and Ni3 Al at 100 K and for Al and Ni at 10 K (after [22])

3.6 Behavior of Defects within the Cascade

151

Fig. 3.21. Number of Frenkel pairs produced per cascade as a function of the PKA energy and irradiation temperature in α -iron (after [22])

In ordered alloys such as Ni3 Al (Fig. 3.20), the Frenkel pair production is similar to that in the pure metal (compare with Ni, for example). In addition to Frenkel pairs, anti-site defects or amorphization can occur in these systems. Anti-site defects consist of atoms of the wrong type occupying regular sites in the sublattice. These anti-site defects are observed to increase with T to the 1.25 power rather than to the 0.75 power as in the case of Frenkel pairs. If the amount of disorder is large enough, amorphization can occur. That the anti-site defects form in the molten core confirm that the thermal spike is important in the formation of these defects. The effect of increasing irradiation temperature on defect production in an ordered structure is to increase the number of anti-site defects, primarily due to the reduced length of focused collision sequences. We now have the description of the damage state that we need in order to begin to describe the development of the physical and mechanical effects of irradiation. The K–P/NRT models along with the energy transfer cross sections provide a means to calculate the number of displacements occurring in a solid from an incident particle of some mass and energy. The spatial, temporal and thermal descriptions of the resulting cascade provide us with a means to estimate the number of defects surviving the cascade quench phase, that are available to influence the microstructure at longer times. To this point, we have focused on developing both a physical and quantitative description of the state of the material at the end of the quench phase of the cascade that is completed within ∼ 10 ps of the initial collision event. From that point forward in time, we will be concerned with the development of the microstructure. This development will continue to occur for weeks, months and even

152

3 The Damage Cascade

years in a reactor core, spanning some 18 orders of magnitude in time, and constitutes the Physical Effects of Radiation Damage, which is the focus of Part II of this text.

Nomenclature A B Cp D Ea Ed ED Ei FD kB m M1 M2 N Nd P(Ei , T ) ri R s T Tˇ Tˆ T¯ Ua Vcas W (λ ) W (Ei , T ) ΔX Y Z Z(T )

βp δ δi,v

Atomic mass; pre-exponential constant in Born–Mayer relation, Eq. (1.47) Constant in exponent in Born–Mayer relation, Eq. (1.47) Specitic heat capacity Thermal diffusivity Energy per atom Displacement energy Damage energy Projectile energy Energy depth distribution Boltzmann’s constant 1/s Mass of projectile Mass of target Atom number density Number of displacements per unit depth Primary recoil spectrum Recombination radius Ion/atom range in the lattice Exponent in power law relationship Energy transferred in collision Minimum energy transferred Maximum energy transferred Average energy transferred Energy per atom Cascade volume Function for distance between primary collisions Weighted primary recoil spectrum Longitudinal moment of the cascade Transverse moment of the cascade Atomic number Fraction of secondary collisions produced above Ed by a PKA of energy T Reduction factor in FPs due to recombination within ri Cascade contraction factor Clustered fraction of vacancies and interstitials

Problems

ε φ γ γi,v η η1 η2 λ ν (T ) νFP Θ σ (E, T ) σD (E) σd σp τ ξ ζ

153

Unit charge Neutron flux 4M1 M2 /(M1 + M2 )2 Isolated point defect fraction Energy lost to electronic excitation in the NRT model; total # free FPs produced in cascade Fraction of defects produced by primary collisions Fraction of defects produced by secondary collisions Mean free path Displacement function Number of Frenkel pairs Cascade energy density Differential energy transfer cross section Displacement cross section for collisions between atoms Total displacement cross section Primary displacement cross section for incident ion Cascade lifetime Displacement efficiency Fraction of vacancies and interstitials initially clustered that are subsequently annihilated in the cascade

Problems 3.1 Plot the mean free path for Ni between the energies of 1 and 10,000 eV, making calculations at each decade. At what energy is the mean free path the smallest? Use Eq. (1.50) to determine the Born–Mayer constants and a value of 40 eV for Ed . 3.2 What is the implication of the difference in shape in the weighted recoil spectra for neutrons and protons in the morphology of the damage cascade? 3.3 For 1 MeV neutrons incident on nickel, determine a) The damage energy b) The effective cascade temperature c) The cascade lifetime using Ua ∼ 0.3 eV and D ∼ 1012 nm2 /s. 3.4 You would like to model displacement cascades. What is the appropriate modeling tool, kinetic Monte Carlo or molecular dynamics? Why? 3.5 Based on your expertise using SRIM, you decide to irradiate a steel sample (Fe–18Cr–9Ni) with nickel ions. You have the choice of examining the sample near the surface of the sample or near the damage peak. You are worried that all the implanted nickel ions will change the local chemistry of the sample. To mitigate this concern, should you look in the region closer to the sample surface or the damage peak? Why?

154

3 The Damage Cascade

References 1. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Service, Springfield, VA 2. Averback RS (1994) J Nucl Mater 216:49 3. Brinkman JA (1956) Amer J Phys 24:251 4. Seeger A (1958) On the theory of radiation damage and radiation hardening. In: Proceedings of the Second United Nations International Conference on the Peaceful Uses of Atomic Energy, Geneva, 1958, Vol. 6, p 250, United Nations, New York 5. Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge 6. Was GS, Allen TR (1994) Mater Character 32:239 7. Sigmund P (1981) Sputtering by ion bombardment: theoretical concepts. In: Behrisch R (ed) Sputtering by Particle Bombardment, Springer, Berlin Heidelberg New York, p 9 8. Heinisch HL (1996) J Metals Dec:38 9. Robinson MT (1994) J Nucl Mater 216:1 10. Robinson MT, Torrens IM (1974) Phys Rev B 9:5008 11. Beeler JR (1966) Phys Rev 150:470 12. Ziegler JF, Biersack JP, Littmark U (1996) The Stopping and Range of Ions in Solids. Pergamon, New York 13. Finnis MW, Sinclair JE (1984) Phil Mag A50:45–55; (1986) Erratum Phil Mag A53:161 14. Calder AF, Bacon DJ (1993) J Nucl Mater 207:25–45 15. Stoller RE (1996) J Metals Dec:23 16. Diaz de la Rubia T, Averback RS, Benedek R, King WE (1987) Phys Rev Lett 59(19):1930 17. Zinkle SJ, Singh BN (1993) J Nucl Mater 199:173 18. Naundorf V (1991) J Nucl Mater 182:254 19. Was GS, Allen TR (2007) In: Radiation Effects in Solids, Sickafus KE, Kotomin EA, Uberoage BP, eds, NATO Science Series, Springer 235:65–98 20. Rehn LE, Okamoto PR, Averback RS (1984) Phys Rev B 30(6):3073 21. Iwase A, Rehn LE, Baldo PM, Funk L (1996) J Nucl Mater 238:224–236 22. Bacon DJ, Gao F, Osetsky YuN (2000) J Nucl Mater 276:1–12 23. Deng HF, Bacon DJ (1996) Phys Rev B 54:11376 24. Calder AF, Bacon DJ (1997) In: Proceedings of Symposium on Microstructure Evolution During Irradiation, Vol. 439. Materials Research Society, Pittsburgh, PA, p 521

4 Point Defect Formation and Diffusion

The first step in understanding the effects of irradiation on materials is to understand, on the atomic level, the nature of radiation damage. In the previous chapters we developed a quantitative description of the process of displacing an atom from its lattice site by the transfer of kinetic energy from a high-energy particle. The recoiling lattice atom travels through the crystal, colliding with its neighbors and displacing these also from their sites. A cascade of atomic collisions is created by the original particle with the end result being a number of vacant lattice sites and an equal number of displaced atoms wedged into the interstices of the lattice. The basic defects (vacancies and interstitials) form the foundation for all observed effects of irradiation on the physical and mechanical properties of materials. Determination of the concentration and diffusion of these basic defects is the subject of this chapter.

4.1 Properties of Irradiation-Induced Defects Various types of defects exist in any crystalline lattice. These include: – – – –

Point defects (0D): vacancies and interstitials Line defects (1D): dislocation lines Planar defects (2D): dislocation loops Volume defects (3D): voids, bubbles, stacking fault tetrahedra

The most basic of these are point defects. Following [1], we will start with interstitials. 4.1.1 Interstitials An interstitial is an atom that is located in a position of a crystal that is not a regular lattice site. There are two broad classifications of interstitial sites in the various cubic crystal lattices: octahedral sites and tetrahedral sites, and these will be briefly reviewed. The fcc lattice is cubic with unit cell of length a (lattice constant) and with atoms located at the corners and the faces of the cube (Fig. 4.1). Each corner atom is shared by eight unit cells and each face atom is shared by two unit cells, so the number of atoms per unit cell is 8 corner atoms ×1/8 atom/unit cell + 6 face atoms ×1/2 atoms/unit cell = 4. Octahedral sites are interstitial positions that are

156

4 Point Defect Formation and Diffusion Fig. 4.1. Face-centered cubic (fcc) lattice unit cell

surrounded by an octahedron where the lattice atoms make up the six vertices of an octahedron. There are four octahedral sites per unit cell in the fcc lattice, the center of the unit cell and the edges. The center site is wholly within the unit cell, but the sites on the edges are each shared by four unit cells (Fig. 4.2a). So the total number of octahedral interstitial sites per unit cell is 1 + 12 edge sites ×1/4 site per unit cell = 4 sites. There are also tetrahedral interstitial sites in the fcc lattice in which the atom is located inside a tetrahedron formed by lattice atoms. These are located in side the corners of the unit cell (Fig. 4.2b). There are a total of 8 tetrahedral sites (one for each corner) in the fcc unit cell. In the bcc lattice, the atoms reside at the corners of the unit cell with one in the center of the cell for a total of two atoms per unit cell; 1 + 8 corner sites ×1/8 site/unit cell = 2 sites (Fig. 4.3). Octahedral interstitial sites are located on the faces and the edges of the unit cell giving 6 faces ×1/2 site per face +12 edges ×1/4 sites

Fig. 4.2. Interstitial positions in the fcc unit cell

4.1 Properties of Irradiation-Induced Defects

157

Fig. 4.3. Body-centered cubic (bcc) lattice unit cell

Fig. 4.4. Interstitial positions in the bcc unit cell

per edge = 6 sites per unit cell (Fig. 4.4a). Tetrahedral interstitial sites are located on the faces and in the corners of the faces. There are 6 faces × 4 locations per face × 1/2 sites/face = 12 tetrahedral sites (Fig. 4.4b). The hcp unit cell is not cubic but rather hexagonal and is defined by the c/a ratio where a is the length of a side of the regular hexagon and c is the height of the cell (Fig. 4.5). There are six atoms per unit cell in the hcp lattice; twelve on the corners shared by six cells (= 2) plus two on the faces shared by two cells (= 1) plus three inside the cell at a height of 1/2c (= 3). There are six octahedral sites per unit cell, all wholly contained within the unit cell (Fig. 4.6a). There are also six tetrahedral sites per unit cell, four wholly contained within the unit cell and six that are shared by each of three cells (Fig. 4.6b).

158

4 Point Defect Formation and Diffusion Fig. 4.5. Hexagonal close packed (hcp) unit cell

Fig. 4.6. Interstitial positions in the hcp unit cell

Our simple picture of interstitials is not a true physical picture because the stable configuration of self-interstitial atoms (SIA) in metals is the dumbbell or splitinterstitial configuration where two atoms are associated with or “share” a single lattice site. Since the atom cores repel each other, the atoms arrange themselves in the lowest energy orientation. This turns out to be with the dumbbell axis along the 100 direction for fcc metals, the 110 direction for bcc metals and the 0001 direction for hcp crystals (Fig. 4.7). To accommodate two atoms in one lattice site, atoms adjacent to the dumbbell are displaced slightly off their lattice positions which then perturbs neighboring atoms and so on. These displacements emanate from the defect, forming an elastic displacement field. The symmetry of the displacement field is reflected by the SIA configuration in the bcc lattice (Fig. 4.8). Consider a 100 dumbbell interstitial configuration in fcc aluminum. The separation distance of the two dumbbells is √ about 0.6a. The nearest neighbor spacing in the fcc lattice is along 110 and is (a/ 2). So the separation distance of a 100 dumbell is about 20% smaller than the nearest neighbor distance in the undistorted lattice. The four nearest neighbors to each dumbbell are displaced outwards by about 0.1a and the total relaxation volume is about 2Ω , where Ω is the atomic volume. The relaxation volume is determined by treating the crystal as an elastic continuum and inserting an atom as an interstitial (or removing one to create a vacancy) and

4.1 Properties of Irradiation-Induced Defects

Fig. 4.7. Configurations of SIAs in (a) fcc, (b) bcc and (c) hcp lattices

Fig. 4.8. Split interstitials in the bcc lattice

159

160

4 Point Defect Formation and Diffusion

Table 4.1. Numerical values, compiled from different sources for some quantities characterizing properties of radiation-induced point defects in metals (from [1]) Symbol Unit Interstitials i Relaxation volume Vrelax Formation energy Efi Equilibrium Ci (Tm ) concentration at Tm∗ i Migration energy Em Vacancies v Relaxation volume Vrelax Formation energy Efv Formation entropy Sfv Equilibrium Cv (Tm ) concentration at Tm∗ v Migration energy Em Activation energy QvSD for self-diffusion Frenkel pairs Formation energy

EfFP

Al

Atomic vol. 1.9 eV 3.2 – 10−18

Cu

Pt

Mo W

1.4 2.2 10−7

2.0 3.5 10−6

1.1

eV

0.12

0.12

0.06

Atomic vol. eV k –

0.05 −0.2 0.66 1.27 0.7 2.4 9 ×10−6 2 ×10−6

eV eV Qa

0.62 1.28

0.8 2.07

1.43 1.3 2.9 4.5

eV

3.9

3.5

5

−0.4 1.51 3.2

0.054

3.8 2 4 ×10−5 1.8 5.7

determining the amount of distortion resulting in the lattice. The high relaxation volumes due to SIAs cause large lattice distortions, which lead to strong interaction with other SIAs and with other lattice defects (dislocation, impurity atoms). The net effect of this elastic interaction is an attraction of mobile SIAs to these defects. Experimental values for the relaxation volume in several metals appear in Table 4.1. 4.1.2 Multiple Interstitials Multiple interstitials form by the agglomeration of mobile SIAs at elevated temperatures. Multiple interstitials have a high binding energy on the order of 1 eV. Since the energy needed to dissociate a SIA from a large cluster approaches the SIA formation energy (2 – 4 eV), SIA clusters are very stable against dissociation at low temperatures. Computer simulation predicts that the stable configuration of a di-interstitial in fcc metals is two parallel dumbbells on nearest neighbor sites (Fig. 4.9). The stable structure of tri-interstitials in fcc metals is predicted by computer simulation to be three orthogonal 100 dumbbells on nearest neighbor sites. The anticipated configuration of di-interstitials in the bcc lattice is two 110 dumbbells on nearest neighbor sites.

4.1 Properties of Irradiation-Induced Defects

161

Fig. 4.9. Di-interstitials in the (a) fcc lattice in stable, metastable and new stable positions, and (b) in the bcc lattice

4.1.3 Interstitial–Impurity Complexes Impurity atoms in metals are efficient traps for SIAs. Stable complexes consisting of undersized atoms and interstitials do not dissociate thermally below a temperature where vacancies become mobile. One possible configuration is the mixed dumbbell where one of the dumbbell atoms is replaced by the impurity atom (Fig. 4.10a). Binding energies are of the order of 0.5 – 1.0 eV. Weaker trapping is observed with oversized impurities (Fig. 4.10b). Interstitial–impurity complexes require only a small activation energy to reorient themselves by so-called cage motion. Shown in Fig. 4.10a, the impurity can jump between the indicated positions of the central octahedron, forming a new mixed dumbbell with the adjacent host atom. Since all of the mixed dumbbells have the impurity end toward the center of the cage, no long-range motion is associated with cage motion. The activation energy of the re-orientation jump in the cage is about 0.01 eV. Movies 4.1 and 4.2 show the behavior of iron and chromium in an Fe–10%Cr alloy following a displacement cascade as a function of the relative sizes of the solutes. In Movie 4.1, chromium is modeled as an oversized solute and in Movie 4.2, chromium is undersized. Note the difference in the interstitial clusters following the cascade cooling period. The undersize Cr (Movie 4.2) undergoes stronger trapping by the iron interstitials than in the case of oversize Cr (Movie 4.1), resulting is a greater number of small interstitial clusters containing Cr.

162

4 Point Defect Formation and Diffusion

Fig. 4.10. (a) Mixed dumbbell configuration in the fcc lattice formed by an undersized impurity and an atom of the host lattice. The vertices of the octahedron are the other locations of the impurity as it makes a dumbbell with the other “face” atoms in the unit cell. (b) Trapping of an interstitial to make a dumbbell with an oversized impurity in the fcc lattice

4.1.4 Vacancies The vacancy, or missing lattice atom, is the simplest point defect in metal lattices. All calculations and computer simulations show that the single vacancy structure is a missing lattice atom with the nearest neighbors relaxing inward toward the vacancy. SIAs have a high formation energy (> 2.0 eV), a large relaxation volume (∼ 2 Ω) and a low migration energy (< 0.15 eV) leading to a high mobility. Vacancies, on the other hand, have low formation energies (< 2 eV), low relaxation volume (0.1 – 0.5 Ω) and high migration energy (> 0.5 eV) and are therefore much less mobile than SIAs (Table 4.1). Further, the strain field of vacancies is isotropic in cubic metals making them hard to investigate. 4.1.5 Multiple Vacancies Multiple vacancies have small binding energies compared to interstitial clusters (0.1 eV) but are often observed in irradiated metals. The configuration of multiple vacancy clusters is shown for the fcc lattice in Fig. 4.11a, and for the bcc lattice in Fig. 4.11b. The migration energy of di-vacancies is less than for single vacancies (0.9 eV vs. 1.32 eV for Ni) but increases with increasing cluster size. It appears that since the tetra-vacancy can only migrate by dissociation, it is the first stable nucleus for further clustering. 4.1.6 Solute–Defect and Impurity–Defect Clusters Vacancies can bind to oversize solute or oversize impurity atoms in order to lower the overall free energy of the solid. Estimates of the binding energy of a vacancy to an oversize solute in the fcc lattice range from 0.2 to 1.0 eV [2]. Hence, these solutes can act as efficient traps for vacancies in the lattice.

4.1 Properties of Irradiation-Induced Defects

Fig. 4.11. Configurations of multiple vacancies in the (a) fcc lattice, and (b) bcc lattice

163

164

4 Point Defect Formation and Diffusion

4.2 Thermodynamics of Point Defect Formation Even in the absence of irradiation, a crystal cannot exist at finite a temperature in a state of absolute perfection. Statistically, there is a finite probability that sufficient energy will be concentrated, by local fluctuations, to form a defect in the crystal lattice. For most purposes, it is fair to assume that the volume of the crystal is constant, for which the Helmholtz free energy function applies. Following [3], if the system is at constant pressure then: F∼ = G = U + pV − T S = H − T S ,

(4.1)

where U is the internal energy, H is the total enthalpy of the N atoms comprising the system. S represents the disorder (entropy) in the system which can be characterized by: S = k ln w ,

(4.2)

where w is the number of possible different configurations of atoms and k is Boltzmann’s constant. Suppose that a crystal has n defects with N available sites. The increase in free energy is: ΔGf = nΔHf − T ΔS ,

(4.3)

where ΔHf is the increase in enthalpy brought about by the introduction (formation) of the defect and ΔS is the change in total entropy, determined as follows. For one defect, there are N available sites and hence N possible configurations. For n defects, there are N for the first, (N − 1) for the second, (N − 2) for the third, etc., up to (N − n + 1) for the nth. This leads to N(N − 1)(N − 2) . . . (N − n + 1) configurations in all. But because these are not all distinct and defects are indistinguishable, the number above allows for n! ways of distributing N defects among n sites. Hence, the number of possible different configurations is: w=

N(N − 1)(N − 2) . . . (N − n + 1) , n!

(4.4)

w=

N! . n!(N − n)!

(4.5)

or

The mixing entropy is then: ΔSmix = k [ln N! − lnn! − ln(N − n)!] .

(4.6)

Using Stirling’s approximation of ln x! x ln x for large x gives: ΔSmix = k ln w ∼ = [N ln N − n lnn − (N − n) ln(N − n)] .

(4.7)

4.2 Thermodynamics of Point Defect Formation

165

In addition to ΔSmix there is a contribution to Δ S from the vibrational disorder of the presence of the defects. According to the Einstein model of lattice motion, the atoms are represented as 3N independent linear harmonic oscillators and the associated entropy is: kT Sf = 3k ln , (4.8) h¯ νE where νE is the natural frequency of the oscillator and h¯ is Planck’s constant. If each defect changes the vibration frequency of z neighbors to νr , the entropy is:

kT kT νE Sf = 3kz ln = 3kz ln + ln , (4.9) h¯ νr h¯ νE νr and for n defects, the total change in entropy due to vibrational disorder is: νE n(Sf − zSf ) = ΔSf = 3nkz ln . (4.10) νr Taking both contributions to the entropy change and inserting them into the free energy equation gives: 3z νE ΔGf = nΔHf − kT N ln N − n lnn − (N − n) ln(n − N) + n ln . (4.11) νr In equilibrium, n will be such that it satisfies dΔGf / dn = 0 giving: ΔHf N − n νE 3z . = ln kT n νr

(4.12)

Assuming n N and letting n/N = C (concentration): C= Writing

νE νr νE νr

3z

−ΔHf exp kT

.

(4.13)

3z in terms of entropy gives the familiar equation:

ΔSf −ΔHf −ΔGf n exp = exp . C = = exp N k kT kt For vacancies we have: v Sf −Efv Cv = exp exp , k kT

(4.14)

(4.15)

166

4 Point Defect Formation and Diffusion

and for interstitials: i S −Efi Ci = exp f exp , k kT

(4.16)

where Efv = ΔHfv and Efi = ΔHfi and Efv , Efi are the formation energies for the respective defect type, and ΔSfv = Sfv , ΔSfi = Sfi . In metals, typical values for Efv are ∼ 1 eV, and for Efi ∼ 4 eV. Hence the formation of vacancies requires considerably less energy than the formation of interstitials (see Table 4.1) and so at thermal equilibrium, Cv Ci . Let us look at an example.

Example 4.1. Calculate the equilibrium concentration of vacancies and interstitials in aluminum at room temperature and 10 ◦C below the melting point. a) RT 20 ◦C or 293 K From Table 4.1, we have: Efv ∼ = 0.66 eV i∼ E = 3.2 eV f

Sfv ∼ 0.7 k Sfi ∼ 8 k ,

and inserting into Eqs. (4.14) and (4.15) yields: Cv = exp (Sfv /k) exp (−Efv /kT ) ∼ 1.6 ×10−11

Ci = exp Sfi /k exp −Efi /kT ∼ 5.0 ×10−51 . b) At 10 ◦C below Tm or 650 ◦C (923 K) Eqs. (4.15) and (4.16) yield: Cv = exp (Sfv /k) exp (−Efv /kT ) ∼ 5.0 ×10−4

Ci = exp Sfi /k exp −Efi /kT ∼ 9.8 ×10−15 .

Besides doing an experiment, how do we go about obtaining an estimate for Efv ? Suppose we create a small cavity in a rigid crystal that has a volume Ω = 4/3π ra3 equal to the volume occupied by one atom, where Ω is the atom volume and ra is the atom radius. Since we must conserve volume, we spread the material from the cavity uniformly over the surface of a crystal. If the crystal is a sphere, we have: R = R + ΔR .

(4.17)

Since the crystal is a rigid medium and volume is conserved: 4π R2ΔR = 4/3π ra3 ,

(4.18)

4.3 Diffusion of Point Defects

167

and if the crystal is large compared to the size of the atom, then R ra and ΔR R and: ΔR = ra3 /3R2 .

(4.19)

If Efv is the difference in surface energy of the crystal with and without a cavity and σ is the surface energy per unit area, then: Efv = 4π ra2 σ + 4πγ (R + ΔR)2 − 4π R2σ

(4.20)

∼ 4πσ (ra2 + 2RΔR)2 , where the first two terms on the right hand side of the equation are the energies associated with the inner and outer surfaces after formation of the vacancy and the last term is the energy of the surface of the crystal before formation of the vacancy, and the ΔR2 term has been neglected. Substituting for ΔR from Eq. (4.19) gives: 2 ra3 v 2 Ef = 4πσ ra + 3R 2 ra 2 = 4πσ ra 1 + , (4.21) 3R and since ra R, we have: Efv ∼ 4πσ ra2 .

(4.22)

In most metals, σ ∼ 10 eV/nm2 and ra ∼ 0.15 nm, so Efv ∼ 2 eV. If we treat the crystal as an elastic continuum, we get a different expression for Efv : Efv = 4π ra2 σ − 12π ra

σ2 σ2 + 6π ra , μ μ

(4.23)

where the first term is the surface energy of the cavity, the second term is the reduction in surface energy due to contraction of the surface by the surface tension, and the third term is the elastic energy stored in the solid, μ is the shear modulus of the crystal, and Efv ∼ 1 eV. Note that an interstitial will cause a displacement that is greater than ra , resulting in a greater formation energy as we have seen already.

4.3 Diffusion of Point Defects Atoms in a lattice are in a constant state of motion due to thermal vibration, and this means that point defects in the lattice are also in motion. The random nature of thermal vibration gives rise to random walk of the atoms via the defects that are in thermal equilibrium with their surroundings, known as self-diffusion. If foreign atoms are present in a pure metal, their diffusion is known as heterodiffusion.

168

4 Point Defect Formation and Diffusion

Self-diffusion arises when a local concentration gradient of defects appears in the crystal, driving atoms to move in the direction that eliminates the gradient. Diffusion is driven by forces other than the concentration gradient, such as stress or strain, electric fields, temperature, etc. Diffusion in a polycrystal is a complex mechanism due to the presence of grain boundaries, internal surfaces, dislocations, etc. We will follow the analysis in [4] by starting with diffusion in a single crystal and then expanding our treatment to include the polycrystalline case later on. 4.3.1 Macroscopic Description of Diffusion Diffusion is governed by two fundamental laws derived by Fick in 1880. They apply to any state of matter due to their general character regarding macroscopic diffusion processes. The first law is a relationship between the flux, J, and the concentration gradient of the diffusing specie: J = −D∇C ,

(4.24)

where D is the diffusion coefficient and ∇C is the composition gradient. For diffusion in one dimension: ∂C . (4.25) J = −D ∂x The minus sign indicates that diffusion takes place in the direction of decreasing concentration of the diffusing specie. D is generally given in units of cm2 /s or m2 /s and for solids between 20 and 1500 ◦C, 10−20 cm2 /s < D < 10−4 cm2 /s. Fick’s second law gives a relation between the concentration gradient and the rate of change of concentration caused by diffusion at a given point in the system:

∂C = −∇ · J = −∇ · D∇C , ∂t which, in one dimension simplifies to ∂C ∂ ∂C =− D . ∂t ∂x ∂x

(4.26)

If D is not a function of the concentration, then we can write Eq. (4.26) as:

∂C = −D∇2C ∂t (4.27) ∂ 2C = −D 2 . ∂x Equations (4.26) or (4.27) can be solved for certain limiting conditions enabling D to be determined on the basis of various measurements. While Fick’s laws provide a description of diffusion on the macroscopic scale, we would like to understand diffusion on the microscopic level as well. Diffusion occurs by several possible mechanisms depending on the nature of the diffusing specie and the host lattice. We will examine these mechanisms and then derive a description of diffusion on the microscopic level.

4.3 Diffusion of Point Defects

169

4.3.2 Mechanisms of Diffusion To obtain a theoretical description of diffusion, we first consider the elementary act of a jump of an atom from one stable position to another in the lattice. There are several mechanisms of lattice diffusion, some requiring the presence of defects, others not. The following types [5] can be distinguished. Exchange and ring mechanisms: The exchange mechanism (Fig. 4.12) consists of the exchange of lattice positions involving two atoms located in adjacent crystal sites. It does not require the presence of defects, and it is highly improbable in close packed crystals since it requires considerable deformation and hence, an enormous activation energy. The ring mechanism (Fig. 4.13) is less energy intensive but requires the coordinated movement of three to five atoms. Since the probability of this is low and the energy required is still high, both the exchange and ring mechanisms are unimportant in crystals containing defects. Vacancy mechanism: This is the simplest mechanism of diffusion and occurs in metals and alloys (Fig. 4.14). Diffusion occurs by the jump of an atom from its lattice site to a vacant site. For an atom to move by this mechanism the presence of a neighboring vacancy is required. Since movement of the vacancy is opposite that of the atom, vacancy-type diffusion is regarded as either a movement of the atom

Fig. 4.12. Exchange mechanism of diffusion

Fig. 4.13. Ring mechanism of diffusion

170

4 Point Defect Formation and Diffusion Fig. 4.14. Vacancy mechanism of diffusion

or the equivalent movement of the vacancy. However, as we will see, the diffusion coefficient for vacancy diffusion is not equal to that for atom diffusion. Interstitial mechanism: This mechanism involves the movement of an atom from one interstitial position to another (Fig. 4.15). It requires considerable energy in order to push its way through the barrier atoms separating the interstitial sites in the crystal (recall the role of barrier atoms in our calculation of displacement energy in Chap. 2). In reality, this mechanism only occurs when the diffusing specie is of an atom type that is smaller than the host lattice atoms. Interstitialcy mechanism: This mechanism involves the displacement of nearby lattice atoms to an interstitial site and generally occurs when atom diameters are comparable. There are two variants of this mechanism: the collinear variant in which displaced atoms move along a straight line (Fig. 4.16a) and the non-collinear variant in which the displaced atom moves to the interstitial position at an angle to the direction of movement of the displacing atom (Fig. 4.16b). Dumbbell interstitial mechanism: This process involves the symmetrical placement of an interstitial and a lattice atom about a single lattice site such that they share the lattice site. Figure 4.17 shows a 2D schematic of the sharing of a single lattice site by two atoms. Recall from our discussion in Sect. 4.1, that the dumbbell is a very stable configuration for the interstitial and that there are preferred directions for the dumbbell that depend on the lattice, and minimize the energy.

Fig. 4.15. Interstitial mechanism of diffusion

4.3 Diffusion of Point Defects

171

Fig. 4.16. Interstitialcy mechanism of diffusion, (a) collinear variant, (b) non-collinear variant

Fig. 4.17. Dumbbell interstitial mechanism of diffusion

Crowding (crowdion) mechanism: This mechanism occurs when an atom is added to a lattice plane but it does not reside in an interstitial position. To accommodate the atom, lattice atoms over, perhaps, 10 lattice constants are all shifted with respect to their lattice sites. The configuration can be thought of as a dumbbell spread over 10 atoms along a row, rather than two (Fig. 4.18). Actually, we have already seen a crowdion in our discussion of focusing collisions. Re-examine Fig. 3.4 and you will see a crowdion emanating from the displacement spike. This configuration is not a stable configuration and exists only temporarily as the energy for the knock-on atoms is expended. Despite the numerous mechanism for diffusion of atoms in a solid, diffusion usually occurs by either the vacancy or interstitialcy mechanisms. Ultimately, we want to obtain a mathematical relation between the macroscopic parameters for diffusion (i.e., the self-diffusion coefficient) and the elementary acts of defect jumps represented by the coefficients of diffusion for defects, or the microscopic process. We will assume that the self-diffusion process consists of a completely random walk of defects, i.e., there is no correlation between successive jumps of the defects. Although this is reasonable for defect diffusion, it is not strictly true for atom diffusion.

172

4 Point Defect Formation and Diffusion Fig. 4.18. Crowdion mechanism of diffusion

As mentioned earlier, jumps of defects and hence, atoms, are due to thermal vibrations of very high frequency. The Debye frequency is ∼ 1013 s−1 . The frequency of atom jumps is orders of magnitude lower, ∼ 108 s−1 at say, 700 ◦C. This means that once every 105 vibrations, a thermal fluctuation is large enough for an atom to overcome the energy barrier separating it from the next stable position. Let us take a closer look at the jumping process. 4.3.3 Microscopic Description of Diffusion Suppose that at time zero, a single impurity atom is placed in a position in a crystal which is designated as the origin. The atom proceeds to jump from one site to another in a completely random manner. Each jump is of distance λ , but since the medium is assumed to be isotropic, each jump is arbitrary and independent of previous jumps. After a time t, the displacement, r, of the particle from the origin is measured. If the experiment is repeated several times, r will not be the same because of the stochastic nature of the process. Rather, the displacements will be distributed according to a function Pt (r) where Pt d 3 r is the probability of finding the atom in a volume element d 3 r a distance r from the origin after time t. The quantity that best describes the extent of migration is the mean square displacement, r2 , which is given by the second moment of the distribution: r2 =

all space

r2 Pt (r)d 3 r = 4π

∞ 0

r4 Pt (r)dr .

(4.28)

We will first compute r2 without knowledge of Pt (r). If the atom makes Γ jumps per unit time, the time interval t corresponds to a number of n jumps given by: n = Γt .

(4.29)

Each jump is represented by a vector λ i , where the subscript, i, refers to the jump number. The vectors are all of the same length, λi , but of random direction. The

4.3 Diffusion of Point Defects

173

Fig. 4.19. Random jump of a defect in an isotropic solid

position of the diffusing atom after n jumps (Fig. 4.19) is the vector sum of the λ i or: r = λ 1 + λ 2 + .λ 3 . . . + λ n .

(4.30)

The magnitude of the square of the displacement is obtained by taking the scalar product of r with itself: r2 = r · r = (λ 1 + λ 2 + .λ 3 . . . + λ n ) · (λ 1 + λ 2 + .λ 3 . . . + λ n ) .

(4.31)

The scalar product of two sums is equivalent to squaring the sums, giving: n

n−1 n

i=1

i=1 j =i

r2 = ∑ λ i · λ i + 2 ∑ ∑ λ i · λ j .

(4.32)

The first term is equal to nλ 2 and the second term can be rewritten as:

λ i · λ j = λ 2 cos θi j ,

(4.33)

and n−1 n

r2 = nλ 2 + 2λ 2 ∑ ∑ cos θi j ,

(4.34)

i−1 j =i

or

r = nλ 2

2

2 n−1 n 1 + ∑ ∑ cos θi j n i=1 j =i

.

(4.35)

The mean square displacement is obtained by averaging r2 over a large number of experiments. The term cos θi j can range from −1 to 1, and by nature of the random hopping process, the average value of cos θi j for any i j combination is zero. Hence, the last term disappears and: r 2 = nλ 2 ,

(4.36)

r2 = λ 2 Γ t .

(4.37)

or

Equation (4.37) relates the mean square displacement to the microscopic properties of jump distance and jump frequency. Now, we wish to compute r2 from a macroscopic viewpoint.

174

4 Point Defect Formation and Diffusion

At t = 0, N impurity atoms are introduced into a restricted region of a host crystal. As a consequence of diffusion (random hopping), the N atoms spread out from the origin in a manner described by C(r,t) which is obtained by solving Fick’s second law (assuming D is not a function of concentration): 1 ∂ ∂C ∂C =D 2 r2 , (4.38) ∂t r ∂r ∂r with initial condition C(r, 0) = 0, for r = 0. Since the N atoms remain in the crystal, C(r,t) is subject to the constraint: ∞ 0

4π r2C(r,t) dr = N ,

(4.39)

with boundary condition that the concentration drops to 0 at infinity, C(∞,t) = 0. The solution to Eq. (4.38) subject to the initial and boundary conditions becomes: exp −r2 /4Dt . (4.40) C(r,t) = N (4π Dt)3/2 The probability of finding the single atom in a spherical shell between r and r + dr after time t, is equivalent (in the macroscopic diffusion description of the problem) to the fraction of the N atoms located in the same volume element after time t. Pr (r) and C(r,t) are related by: C(r,t) exp −r2 /4Dt = . (4.41) Pt (r) = N (4π Dt)3/2 The mean square displacement is: r 2 = 4π

∞ 0

r4 Pt (r) dr

4π = (4π Dt)3/2

∞ 0

r4 exp −r2 /4Dt ,

(4.42)

or r2 = 6Dt .

(4.43)

Comparing to r2 = λ 2Γ t from our microscopic solution Eq. (4.37), we have: D = 1/6λ 2Γ ,

(4.44)

which is the Einstein formula and is the link between the microscopic diffusion parameters λ and Γ , and the macroscopic diffusion parameter, D. 4.3.4 Jump Frequency, Γ We define Γ as the total number of jumps per second for an atom. Therefore, in a time increment δ t, we expect Γ δ t jumps. The quantity Γ δ t is proportional to z,

4.3 Diffusion of Point Defects

175

the number of nearest neighbors (sites), pv , the probability that a given neighboring site is vacant, and ω , the frequency with which an atom jumps to a particular site. Thus, the frequency with which an atom jumps to any neighboring equilibrium site, Γ , is the product of the jump frequency to a single site, ω , the number of nearest neighbor sites, z, and the probability that one site is vacant, pv , or:

Γ = zpv ω ,

(4.45)

Dva = 1/6zλ 2 pv ω .

(4.46)

and

where we have properly included the subscript a and superscript v to indicate that this is the diffusion coefficient for atom diffusion via vacancies. Also note that the jump distance λ is related to the lattice constant by λ = Aa, where the coefficient, A, depends on the diffusion mechanism and the crystal structure. The terms 1/6zA2 are often lumped together into a single parameter, α , such that: Dva = α a2 pv ω ,

(4.47)

and if vacancy motion is random, then pv = Nv and: Dva = α a2 Nv ω .

(4.48)

Let us look at an example of how to determine α for a specific diffusion process and crystal structure.

Example 4.2. Vacancy diffusion in the bcc and fcc lattices In the case of the vacancy mechanism of diffusion in a bcc structure, each atom√has eight nearest neighbors (z = 8). The jump distance is related to a by A = 23 , and hence, α = 1. For the simple interstitial diffusion mechanism in a bcc lattice, z = 4 and A = 1/2 giving α = 1/6. For the fcc lattice, z = 12 and A = √12 , giving α = 1. For interstitials in the fcc lattice, z = 12 and A = 1/2 and α = 1/2. Before continuing, it is instructive to point out the difference between vacancy diffusion and atom diffusion via a vacancy mechanism (vacancy self-diffusion). In determining the components of Γ , we noted that Γ depends on the probability, pv , that a neighboring lattice site is vacant. This is a necessary condition for an atom jump via a vacancy. However, if we are following the migration of the vacancy, then Γ depends on the probability that a neighboring lattice site to the vacancy is filled by an atom. Since in all but the most extreme cases, this probability is ∼ 1, and the equation for vacancy diffusion is given as follows: Dv = α a 2 ω , and differs from that for vacancy self-diffusion by the factor Nv .

(4.49)

176

4 Point Defect Formation and Diffusion

4.3.5 Jump Frequency, ω In calculating ω we will ignore detailed atomic movements and instead deal in terms of “activated complexes” or regions containing an atom midway between two equilibrium sites (Fig. 4.20). The number of atoms diffusing per second is then obtained by multiplying the number of activated complexes (nm ) by the average velocity of the atoms moving through this barrier (ν¯ ) divided by the width of this barrier (δ ). The jump frequency is then:

ω=

Nm ν¯ , δ

(4.50)

where Nm is the mole fraction of activated complexes. The work done in moving an atom across this barrier is equal to the change in Gibbs free energy for the region, ΔGm : ΔGm = ΔHm − T ΔSm .

(4.51)

Using ΔGm , the equilibrium mole fraction of atoms in the region of the saddle point in Fig. 4.20, Nm can be calculated in the same way we calculated Nv . Instead of mixing vacancies to raise the free energy by ΔGv per mole, we are mixing complexes to raise the free energy an amount ΔGm per mole. The ideal entropy of mixing is the same for vacancies as for complexes so, at equilibrium, nm out of N atoms will be in the neighborhood of the saddle point at any instant and: −ΔHm + T ΔSm nm −ΔGm = Nm = exp = exp . N kT kT

(4.52)

Nm ν¯ and ν¯ /δ is the frequency (call it ν ) at which atoms at From Eq. (4.50), ω = δ the saddle point jump to the new site. Thus Nm ν out of N atoms will jump from one

Fig. 4.20. Passage of the “activated complex” from one stable position, through a saddle point, to another stable position

4.3 Diffusion of Point Defects

site to a given site per second, and the average jump frequency is: −ΔGm ΔSm nm ν −ΔHm = ω = ν exp = ν exp exp N kT k kT Sm −Em = ν exp exp , k kT

177

(4.53)

where ν is the Debye frequency (∼ 1013 s−1 ) and Em = ΔHm and Sm = ΔSm . 4.3.6 Equations for D We are now in a position to write the expressions for the diffusion coefficients for the motion of the defects, and of the atoms by way of the defects: 1. The vacancy diffusion coefficient is given by: Dv = α a 2 ω where

ω = ν exp

−ΔGvm kT

= ν exp

then

Sv Dv = α a ω = α a ν exp m k 2

2

v Sm k

exp

v −Em exp kT

v −Em kT

,

(4.54)

2. The vacancy self-diffusion coefficient is the product of the vacancy diffusion coefficient and the probability that the nearest neighbor site is vacant, Nv : Dva = α a2 Nv ω , where NV = exp

−ΔGvf kT

giving:

Dva = α a2 ν exp

= exp

Sfv k

exp

Efv kT

,

v Sfv + Svm −Efv − Em exp . k kT

(4.55)

3. The interstitial diffusion coefficient is: Di = α a 2 ω , or

Di = α a2 ν exp

i Sm k

exp

i −Em kT

.

(4.56)

178

4 Point Defect Formation and Diffusion

4. The interstitial self-diffusion coefficient is the interstitial diffusion coefficient times the probability that a neighboring site contains an interstitial, Ni : Dia = α a2 Ni ω , where

Ni = exp

−ΔGif kT

giving

= exp

Sfi k

exp

−Efi kT

,

i i Sfi + Sm −Efi + −Em exp . (4.57) k kT The diffusion coefficients are all different in detail, but similar in form as they consist of two factors; a constant that is independent of temperature and an exponential of temperature containing an energy term. All equations for D can be rewritten in the form: (4.58) D = D0 exp(−Q/kT ) , where D0 = α a2 ν is the temperature independent term and Q is the activation energy. For vacancy diffusion we have: v Qv = E m , (4.59) and for vacancy self-diffusion we have: v Qva = Efv + Em . (4.60) For interstitials we have: i and Qi = Em , (4.61) and for interstitial self-diffusion we have: i Qia = Efi + Em . (4.62) It follows that the activation energy for diffusion of atoms in a crystal depends on both the energy of formation of defects and the energy required for their migration in the periodic field of the crystal lattice. Experiments can be conducted to confirm the temperature dependence of D and also the values of Q. The terms in the pre-exponential factor for the various diffusion mechanisms are provided in Table 4.2 for the fcc and bcc lattices. Dia = α a2 ν exp

Example 4.3. Determination of Dva and Dia for fcc copper at 500 ◦C For copper: Efv = 1.27 eV ,

Efi = 2.2 eV

v = 0.8 eV , Em

i Em = 0.12 eV

Sfv = 2.4 k ,

Sfi

v and Si . and we neglect Sm m

∼0

4.3 Diffusion of Point Defects

179

√ For the fcc lattice, z = 12, A = 1/ 2, and a ∼ 3 nm, giving: −0.8 2 Dv = α a ν exp kT −6 2 ∼ cm /s 5 ×10 = −0.12 2 Di = α a ν exp kT −2 2 ∼ = 7 ×10 cm /s Dva = α a2 ν exp

2.4k −1.27 − 0.8 exp k kT

∼ = 3 ×10−13 cm2 /s −2.2 − 0.12 i 2 Da = α a ν exp kT −16 2 ∼ 3 ×10 cm /s = Note that while Di /Dv ∼ 104 due to the smaller migration energy for interstitials than for vacancies, but Dia /Dva ∼ 10−3 because of the very high interstitial formation energy compared to that for vacancies. Plots of the diffusion coefficients are shown in Fig. 4.21. Note that the vacancy diffusion coefficient is larger than the vacancy self-diffusion coefficient and has a smaller slope.

Table 4.2. Parameters in the expression for the diffusion coefficient, D = α a2 N ω , where α = 1/6zA2 for the various diffusion mechanisms in the fcc and bcc lattices Diffusion mechanism

z

A

α

N

D

Vacancy Vacancy self-diffusion Interstitial Interstitial self-diffusion

12 12 12 12

fcc√ 1/√2 1/ 2 1/2 1/2

1 1 1/2 1/2

1 Nv 1 Ni

a2 ω a2 Nv ω 1/2a2 ω 1/2a2 Ni ω

Vacancy Vacancy self-diffusion Interstitial Interstitial self-diffusion

8 8 4 4

bcc √ √3/2 3/2 1/2 1/2

1 1 1/6 1/6

1 Nv 1 Ni

a2 ω a2 Nv ω a2 ω 1/6a2 Ni ω

180

4 Point Defect Formation and Diffusion Fig. 4.21. Comparison of plots of ln D vs. 1/T for vacancy diffusion and vacancy selfdiffusion

The behavior of self-interstitial atoms in bcc iron at 323 ◦C is illustrated in Movie 4.3. In this movie, the green balls are the interstitials and the red ball is the vacant lattice site, and together they form a SIA dumbbell in which the two green atoms share a single lattice site. The SIA originates as a 110 split-dumbbell interstitial and then rotates into a 111 interstitial and moves in one-dimension through the 111 crowdion saddle position. Movie 4.4 shows a di-SIA consisting of two parallel 111 split-dumbbells that migrates along the 111 direction and also rotates to different 111-type orientations.

4.4 Correlated Diffusion Earlier we assumed that irrespective of the kinds of defects present in a crystal lattice, successive jumps of atoms are completely random or uncorrelated. This means that after n jumps, all possible directions for the (n + 1)th jump are equally probable. This is true for vacancies or interstitials since all structural elements surrounding them are at all times identical. Since the vibrational frequency of a lattice atom is several orders of magnitude greater than the jump frequency, equilibrium in the region surrounding the defect is rapidly established between successive jumps and the next jump occurs with no effect of the previous jump on its direction. But this does not always hold true for atom diffusion as described in [5] and in the following. If we consider the case of a radioactive tracer to track atom diffusion, a tracer will make a jump if a vacancy is in its immediate vicinity. The second jump is uncorrelated with the first if the probability of the second jump is the same for all directions. However, the tracer arrives from a position that is vacant at the time of its arrival. Hence, when it is “preparing” for the next jump, the chance that the position from which it has arrived is unoccupied is greater than for any other position around the atom. The two jumps are correlated since the probability of the tracer returning to its former position is higher than for making a jump in any other direction. In

4.4 Correlated Diffusion

181

other words, the tracer has a greater tendency to move in the direction from which it came than in the direction it is headed, or from Eq. (4.35), cos θ 2 < 0. Since jumps in the direction from which it came are most probable, the tracer will have traveled a shorter (net) distance than that traveled by the vacancy. Therefore, the self-diffusion coefficient of the tracer (which is a measure of the rate of this process) is smaller than that of the atoms constituting the lattice, since the self-diffusion of the tracer is a correlated random walk whereas the movement of the vacancies and consequently of the atoms constituting the lattice are not correlated. The correlation effect is absent in the simple interstitial mechanism, but there is correlation of motion by the interstitialcy mechanism. In both the vacancy and the interstitialcy mechanisms, Dtracer < Dlattice and: f=

Dtracer , Dlattice

(4.63)

and f is known as the Haven coefficient and is a measure of the degree to which diffusion is random. Recall our earlier discussion of the measurement of the square of the displacement by random walk given by Eq. (4.35): 2 n−1 n 2 2 r = nλ 1 + ∑ ∑ cos θi j , n i=1 j =i where the mean square displacement is obtained by averaging over all values of cos θi j . In this expression the term in brackets is f and the value of f for random walk is 1 since the average over all cos θi j is 0. But when there is correlation between successive jumps, f is = 1. For the vacancy mechanism of diffusion of a tracer in a regular lattice [5]: fv =

1 + cos θ , 1 − cos θ

(4.64)

and for interstitial diffusion, fi = 1 + cos θ .

(4.65)

Since in both cases, cos θ < 0, then f < 1. 1−P , where P is the probability of a jump A simpler treatment of fv is that fv = 1+P of a tracer to a neighboring vacancy, and 1 − P is the probability that a neighboring vacancy will move away as a result of jumps of lattice atoms. To a first approximation, P is equal to the reciprocal of the number of nearest lattice sites, z, around the tracer. Therefore: f=

1 − 1/z z − 1 = . 1 + 1/z z + 1

(4.66)

182

4 Point Defect Formation and Diffusion

For the fcc lattice: f=

1 − 1/12 12 − 1 = = 0.85 . 1 + 1/12 12 + 1

For the bcc lattice: f=

1 − 1/8 8 − 1 = = 0.78 . 1 + 1/8 8 + 1

For the simple cubic (sc) lattice: f=

1 − 1/6 6 − 1 = = 0.71 . 1 + 1/6 6 + 1

So, in our microscopic description of the diffusion coefficient D, Eq. (4.44), we account for correlated diffusion by including the correlation coefficient: D = 1/6 f λ 2Γ = f α a2 ω .

(4.67)

As an aside, the true correlation coefficient, f , actually consists of two terms, f and f such that f = f f . The quantity f was described in the previous section (as f ) and f is related to the difference between the distances traveled during the elementary act by the tracer atom and the defect: f =

λtracer , λdefect

(4.68)

In the case of a vacancy, f = 1 since λtracer = λvacancy , or the distance traveled by the tracer and the defect are equal in one jump. The same is true for the simple interstitial mechanism. But in the case of the interstitialcy mechanism, the tracer moves from an interstitial position to a lattice site (or vice versa). In both cases, it travels a distance λtracer . However, the passage of a lattice atom from an interstitial position to a lattice site is equivalent to the appearance of an identical atom displaced from the lattice site in a neighboring interstitial position. Therefore, the jump of a lattice atom from the interstitial position to a lattice site requires (for the collinear case) a displacement of the lattice atom by a distance 2λtracer , or f = λtracer /2λtracer = 0.5. For the noncollinear case, f = λtracer /1.6λtracer = 2/3. Table 4.3 summarizes the correlation coefficient for various diffusion mechanisms in the common crystal lattices.

4.5 Diffusion in Multicomponent Systems Our discussion on diffusion so far has applied only to pure or single-component systems. We have not accounted for multiple components such as impurities in a pure metal and alloys. Diffusion in these systems was treated in experiments conducted by Smigelskas and Kirkendall in 1947 [6] and analyzed by Darken in 1948 [7]. The

4.5 Diffusion in Multicomponent Systems

183

Table 4.3. Correlation coefficients for the most common diffusion mechanisms in the various crystal lattices (from [5]) Crystal lattice

Diffusion mechanism

Correlation factor

Simple cubic

Vacancy Interstitial Collinear Non-collinear Vacancy Interstitial Collinear Non-collinear Vacancy Vacancy

0.65311

Face-centered cubic

Body-centered cubic Hexagonal close packed

0.80000 0.96970 0.72722 0.66666 0.72740 0.72722 0.78121

result is that the diffusion coefficients of the two components in a binary (A–B) system can be expressed as: D˜ = DA NA + DB NB ,

(4.69)

where DA,B are the intrinsic diffusion coefficients and are functions of composition, and D˜ is the interdiffusion coefficient. Since the partial diffusion coefficients depend on the alloy composition, D˜ is a complex, non-linear function of concentration. However, in the case of dilute solutions (NB → 0, NA → 1), the interdiffusion coefficient is approximately equal to the partial diffusion coefficient of the solute. The significance of this result can be appreciated by a brief review of the elegance and implications of the experiment. In Kirkendall’s experiment, molybdenum wires were wound around a block of brass (70Cu–30Zn) which was then plated with a thick coating of copper. The molybdenum wires are insoluble in copper and act as inert markers to locate the original interface. When the assembly is heated in a furnace, the wire markers on opposite sides of the brass moved toward each other, indicating that more material has left the brass than entered it, implying that the diffusion coefficient of zinc is greater than that of copper. The vacancy mechanism is the only diffusion mechanism that can account for marker motion. If zinc diffuses by a vacancy mechanism, then the flux of zinc atoms in one direction must equal the flux of vacancies in the opposite direction and the number of zinc atoms leaving the brass is balanced by an equal number of vacancies entering the brass. But the vacancies are absorbed by internal sinks, so the result is that the volume of the brass diminishes and the markers move closer together. The concept of a flux of atoms giving rise to a flux of defects will be explored in depth in Chap. 6 on Radiation-Induced Segregation, which occurs by the inverse Kirkendall effect.

184

4 Point Defect Formation and Diffusion

4.6 Diffusion along High Diffusivity Paths Metals and alloys used as structural engineering materials are polycrystals and are thus, inhomogeneous, as they contain grain boundaries, dislocations, internal interfaces due to precipitates or second phases, etc. To understand diffusion in these systems, we must discuss the effect of these linear, planar and area defects on the diffusion process. The primary difference between mono- and polycrystals is that the latter consists of aggregates of crystals oriented (generally) at random. This latter type of structure rarely shows anisotropy of diffusion. The important difference is that linear and planar defects represent high diffusivity paths along which diffusion can occur much faster than via point defects (bulk diffusion). Grain boundaries are important high diffusivity paths since the atom packing density is lower. There exist several models of grain boundary diffusion, and all assume that the boundary has of width, δ ∼ 0.3 –0.5 nm. One model that is based on the dislocation model of grain boundaries deserves special attention. In this model, the grain boundary is regarded as a number of edge dislocations. The dislocation density (#/unit length) increases with increasing misorientation angle θ , between two grains in contact (Fig. 4.22). From the figure: d sin

b θ = . 2 2

(4.70)

Hence, the distance between neighboring dislocations decreases with increasing misorientation angle. A low angle grain boundary consisting of many edge dislocations can be regarded as a row of parallel channels in which packing of atoms is loosest. In this region, the strain is high and the packing of atoms is loose, and the diffusion coefficient will be the highest along the dislocation lines (cores). According to this model, diffusion along grain boundaries should be anisotropic, and depend on the angle θ . The grain boundary described as a slab of uniform thickness δ and diffusion coefficient Dgb , can also be viewed as a planar array of pipes of radius p and spacing d. Grain boundary diffusion is related to diffusion along dislocation cores (also known as pipe diffusion), described by Dp , by the following relation: Dgb δ = Dp (π p2 /d) ,

(4.71)

and substituting for d from Eq. (4.70) gives: 2 2 sin θ /2 = Dp π p b Dp π p 2 θ ∼ . = b

(4.72)

The dislocation model of the grain boundary shown in Fig. 4.22 is expanded in Fig. 4.23 to show that the extra half planes of atoms can be regarded as edge dislocations. In fact, the rate of diffusion along the grain boundary increases with increasing misorientation angle, θ , and reaches a maximum at θ = 45◦ (Fig. 4.24).

4.6 Diffusion along High Diffusivity Paths

185

Fig. 4.22. Dislocation model of a small angle grain boundary and the geometrical relationship between the angle of tilt, θ , the Burgers vector, b, and the spacing between the dislocations, d

Fig. 4.23. Expanded view of the dislocation model of the grain boundary shown in Fig. 4.22

186

4 Point Defect Formation and Diffusion

Fig. 4.24. Effect of grain boundary misorientation angle on the diffusion of atoms along grain boundaries (after [5])

At angles greater than 45◦ , the dislocation model of grain boundaries breaks down since the distance between dislocations, d, would have to be smaller than the lattice constant. This result also indicates that there should be a relationship between the mean ¯ in a polycrystalline material and the grain value of the diffusion coefficient, D, size, d, since as the grain size decreases, the grain boundary area per unit volume increases. Therefore, D¯ should increase with decreasing grain size as shown in Fig. 4.25. We can write the diffusion coefficient of a solid in which diffusion occurs by bulk diffusion (vacancy mechanism) and grain boundary diffusion as: −Qgb −Qva v ¯ + Dgb exp , (4.73) D = Da exp kT kT where Dva and Qva refer to vacancy self-diffusion and Dgb and Qgb refer to grain boundary diffusion. In most metals, Qva ∼ 2Qgb , so at low temperature, grain boundary diffusion dominates and at high temperature, diffusion is dominated by bulk, or volume diffusion (Fig. 4.25). Pipe diffusion along dislocation cores can also influence low temperature lattice diffusion and the total diffusion coefficient can be estimated simply by: D¯ = f Dp + (1 − f )Dva ,

(4.74)

where D¯ is the mean diffusion coefficient, Dp is the diffusion coefficient for dislocations and Dva is the self-diffusion coefficient and f is the fraction of time that the diffusing atom spends within the dislocation. As the dislocation density increases, f increases, and since Dp > Dva , then D increases as well.

Nomenclature

187

Fig. 4.25. The effect of grain size on the character of diffusion in polycrystalline solids

This general formulation can also be applied to interface or surface diffusion occurring on external and internal surfaces of solids. In general, for defects in the lattice, the more loosely bound the atoms, the lower is the activation energy and the higher is the diffusion coefficient. So surface diffusion requires a lower activation energy than that for other forms of diffusion since each surface atom has only half the nearest neighbors as it does in the bulk, and generally: Qsurface < Qgb < Qp < Qva ,

and so

Dsurface > Dgb > Dp > Dva .

Nomenclature a A C Dyx Dgb D˜ Dlattice Dp Dtracer E f F G H J k n nm N pv P

Lattice constant Factor depending on geometry and diffusion mechanism Concentration Diffusion coefficient of species x via y Diffusion coefficient for grain boundary diffusion Interdiffusion coefficient Diffusion coefficient of lattice atom Diffusion coefficient for pipe diffusion Diffusion coefficient of tracer atom Energy Correlation (Haven) coefficient Helmholtz free energy Gibbs free energy Enthalpy Flux [cm−2 ] Boltzmann’s constant Number of defects Number of activated complexes Number of sites Probability that a lattice site is vacant Pressure

(4.75)

188

4 Point Defect Formation and Diffusion

Q R ra S T U ν¯ V z

α δ γ Γ Λ μ ν νE νr σ ω Ω

Activation energy Radius Radius of an atom Entropy Temperature internal energy Average velocity of atoms moving through barrier in activated complex, Eq. (4.50) Volume Number of nearest neighbors 1/6zA2 Width of the barrier in an activated complex Eq. (4.50); grain boundary width Stacking fault energy Jump frequency Jump distance Shear modulus Frequency; Poisson’s ratio Natural frequency of an oscillator Perturbed frequency of an oscillator Surface energy Jump frequency to a single site Volume of an atom

Subscripts a E f gb i,v m p r th

Atomic Natural component to ν Formation Grain boundary Interstitials, vacancies Migration Pipe Vibrational contribution to ν Thermal

Superscripts FP i,v mix

Frenkel pair Interstitials, vacancies Mixing

Acronyms SIA

Single interstitial atom

Problems

189

Problems 4.1 Many metals occur with both bcc and fcc structure, and it is observed that the transition from one structure to the other involves only insignificant volume change. Assuming no volume change, find the ratio Dfcc /Dbcc where Dfcc and Dbcc are the closest distances between metal atoms in the respective structures. 4.2 For a Ni lattice, calculate the following parameters for atomic chains along the (110) direction: a) the number of atoms per unit chain length b) the number of chains per unit area c) the product of the two. What is this product? 4.3 In the past, investigators have sometimes considered an interstitial atom as having been produced by the transfer of an atom from a normal lattice site to an interstitial site, thus resulting in a one-to-one correspondence between the concentrations of vacancies and interstitials. However, the equilibrium number of vacancies is generally orders of magnitude greater than the equilibrium number of interstitials at a given temperature. Explain. 4.4 The magnitude of the relaxation volume, |V | is greater than 1.0 for interstitials and is less than 1.0 for vacancies. Explain. 4.5 In terms of the jump frequency to a particular neighboring site, ω , and the lattice constant, a, what is the diffusion coefficient for impurity atoms whose equilibrium position is the octahedral interstitial site in: a) the fcc lattice b) the bcc lattice? 4.6 Consider a rigid crystal in the shape of a sphere of radius R. We create a small cavity of radius r (one atomic volume) in the center of the sphere. The material that was in this volume is spread uniformly over the surface of the sphere (assuming this can be done), increasing the radius of the sphere to R . a) Show that for an atomic radius of 0.15 nm and an intrinsic surface energy, σ ∼ 10 eV/nm2, the formation energy of a vacancy is of order 2 eV. b) If instead of a rigid solid, the crystal is treated as an elastic continuum, how would this affect the value of Efv you calculated for part (a)? Why? 4.7 Calculate the diffusivity of interstitials and vacancies in a piece of copper at 484 ◦C. Neglect the contributions of mixing entropy. Use 0.361 nm for the lattice constant. Also, calculate the diffusion coefficient for diffusion of atoms by vacancy self-diffusion. Why is this so much lower than the diffusivity of vacancies? Take γ = 1. 4.8 In a laboratory experiment conducted at 10 ◦C below the melting point of copper, 0.02% of the atom sites are vacant. At 500 ◦C, the vacant atom fraction was 5.7 ×10−8. a) What is the vacancy formation energy? b) How many vacancies are there per cm3 at 800 ◦C?

190

4 Point Defect Formation and Diffusion

References 1. Ullmaier H, Schilling W (1980) Radiation damage in metallic reactor materials. In: Physics of Modern Materials, vol. I. IAEA, Vienna 2. Hackett MJ, Was GS, Simonen EP (2005) J ASTM Int 2(7) 3. Thompson MW (1969) Defects and Radiation Damage in Metals. Cambridge University Press, Cambridge 4. Shewmon PG (1989) Diffusion in Solids. The Minerals, Metals and Materials Society, Warrendale, PA 5. Mrowec S (1980) Defects and Diffusion in Solids, an Introduction. Elsevier, New York 6. Smigelskas A, Kirkendall E (1947) Trans AIME 171:130 7. Darken L (1948) Trans AIME 175:184–201

5 Radiation-Enhanced Diffusion and Defect Reaction Rate Theory

We have developed an understanding of the formation of point defects, their motion or diffusion in a solid, and the configurations of some of the common types of defect clusters encountered in irradiated and unirradiated metals. Clearly, the formation, growth and dissolution of defect aggregates such as voids, dislocation loops, etc., depend upon the diffusion of point defects and their reaction with the defect aggregates. But they also depend upon the concentration of point defects in the solid. The concentration at any point and time is a balance between the production rate, and the loss rate of point defects and is adequately described by the point defect balance equations. The increase in diffusion or enhancement of atom mobility in an irradiated metal is due to two factors: (1) the enhanced concentration of the defects, and (2) the creation of new defect species. Recall that the diffusion of lattice atoms by way of the vacancy mechanism is given by: Dva = fv DvCv , where Dv is the vacancy diffusion coefficient, Cv is the vacancy concentration and fv is the correlation coefficient. Thus, increasing the concentration of vacancies will increase the diffusion coefficient for the atoms in the metal. However, if other mechanisms of diffusion are operative, such as interstitials or di-vacancies, then the total diffusion coefficient for atoms, Da is written as: Da = fv DvCv + fi DiCi + f2v D2vC2v + . . . and diffusion of atoms in the metal is increased by opening new channels via defect species which are usually not present in significant concentration at thermal equilibrium. Under irradiation, Da is also written as Drad . In this chapter, we will develop the transient and steady state solutions to the point defect balance equations in different temperature and microstructural regimes within the framework of radiation-enhanced diffusion [1, 2]. The solutions to the equations are used to determine the radiation-enhanced diffusion coefficient. Reaction rate theory is then presented to develop an understanding of how point defects interact with the various defect aggregates. Radiation-enhanced diffusion and defect reaction rate theory are essential to understanding the evolution of the irradiated microstructure developed in Chaps. 6–10.

192

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.1 Point Defect Balance Equations The development of radiation-induced vacancy and interstitial concentrations occurs due to competing processes. Frenkel defects are created from the collisions between high-energy particles and lattice atoms. These defects can be lost either through recombination of vacancies and interstitials or by reaction with a defect sink (void, dislocation, dislocation loop, grain boundary or precipitate). The local change in defect concentration of the various defect species can be written as the net result of (1) the local production rate, (2) reaction with other species, and (3) diffusion into or out of the local volume or the divergence of the flow. The main reactions we will focus on in this treatment are vacancy–interstitial recombination (v + i → , where represents a lattice site) and point defect reactions with sinks (v + s → s, and i + s → s). These competing processes can be mathematically described by the chemical rate equations: dCv = K0 − KivCiCv − KvsCvCs dt dCi = K0 − KivCiCv − KisCiCs , dt where Cv = vacancy concentration Ci = interstitial concentration K0 = defect production rate Kiv = vacancy–interstitial recombination rate coefficient Kvs = vacancy–sink reaction rate coefficient Kis = interstitial–sink reaction rate coefficient

(5.1)

The terms Kiv , Kvs , Kis are rate constants of the general form, K jX that describe the loss rate of point defects, j per unit point defect concentration to sinks of type, X. Similar equations can be written for defect agglomerates such as di- and trivacancies and interstitials. Note that the equations are non-linear differential equations and they are not mutually symmetric with respect to vacancy and interstitial concentrations because of the difference in Kis and Kvs , making an analytical solution difficult. The term “chemical” refers to homogeneous reactions, where the rate depends only on concentration (“law of mass action”) and not on the local distribution C(r) of the reactants. Thus, uniformity and thereby chemical kinetics require that ∇C ≈ 0. This gives rise to a problem when considering localized sinks, e.g., dislocations, grain boundaries, voids, precipitate interfaces, etc. Such local sinks violate the supposition of spatial uniformity in the host metal in that there is now locally, a directed net flow of mobile point defects toward the closest sinks. The divergence of the flow is equivalent to another “reaction” term, ∇ · D∇C in the kinetic balance equations. The locally valid rate equations are:

∂ Cv = K0 − KivCiCv − KvsCvCs + ∇ · Dv∇Cv ∂t ∂ Ci = K0 − KivCiCv − KisCiCs + ∇ · Di∇Ci . ∂t

(5.2)

5.1 Point Defect Balance Equations

193

The solution to these equations requires the statement of boundary conditions in addition to the initial local concentrations of the mobile defects (vacancies and interstitials). However, we can assume that ∇C ≈ 0 if the mean defect separation is greater than the mean distance between sinks, that is, the sink density is higher than the defect density. This amounts to treating the sink as being uniformly distributed and Eq. (5.1) applies. We consider the following model for the solution to Eq. (5.1). A pure metal is irradiated to produce only single vacancies and single interstitials in equal numbers with no spatial correlation of the interstitial with its vacancy. The interstitials and vacancies migrate by random walk diffusion, annihilating each other by mutual recombination or at unsaturable fixed sinks. Sinks and defects are distributed homogeneously in the metal. The diffusion coefficient of the metal is given by the sum of terms due to its diffusion by vacancies and interstitials. The model will have the following limitations: 1. The model applies to a pure metal. Binding of defects to atomic species and limitation of defect motion due to binding and correlation effects are neglected, f = 1. 2. The sink concentrations and strengths are time-independent, or unsaturable. 3. Other than mutual recombination, defect–defect interactions (e.g., the formation of di-vacancies or di-interstitials) are ignored. 4. Bias factors for diffusion of defects to sinks are set to unity (no preferential absorption of specific point defects at specific sinks). 5. Diffusion terms in and out of a specific volume are not considered. 6. The thermal equilibrium vacancy concentration is neglected. The rate constants are as follows: Kiv = 4π riv (Di + Dv) ≈ 4π riv Di

(5.3)

since Di Dv , Kis = 4π ris Di

(5.4)

Kvs = 4π rvs Dv ,

(5.5)

where riv , rvs and ris are interaction radii for the reaction between the species given by the subscripts and represent the radii of surfaces such that if crossed by the defect, it is annihilated. The terms Di and Dv are the interstitial and vacancy diffusion coefficients, respectively. The production term, K0 , is the effective point defect production rate in that it refers to the production of only freely migrating defects that can give rise to long-range diffusion (see Chap. 3). The derivations of the terms in Eqs. (5.3) and (5.4) will be given in the Sect. 5.3. Note that since the rate constants can differ by several orders of magnitude, the equations are stiff. That is, the time increment needed to follow interstitial motion is orders of magnitude too small to show any vacancy motion. Therefore, the equations must be solved using numerical techniques for stiff equations. But we can gain

194

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

insight into the processes by looking at analytical solutions to limiting cases. For example, the defect concentrations initially increase linearly with Cv = Ci = K0t. Further development depends on the values of the temperature and sink concentration, Cs . We will develop analytical solutions to Eq. (5.1) for four different regimes (combinations of T and Cs ); (1) low T and low Cs , (2) low T and intermediate Cs , (3) low T and high Cs , and (4) high T . 5.1.1 Case 1: Low Temperature, Low Sink Density The approximate solutions to Eq. (5.1) for low temperature and low sink density are given in Fig. 5.1. Initially, defect concentrations build up according to dC/dt = K0 with Ci ∼ Cv , so Ci = Cv = C = K0t. Initially, the concentrations are too low for either recombination or sinks to have an effect on the buildup. The buildup of point defects will start to level off when the production rate is compensated by the recombination rate. In the time regime where the production rate is balanced by the recombination rate, we drop the last two terms from Eq. (5.1) and solve for the “quasi-steady state” concentrations: dC = K0 − KivC2 = 0 (C = Ci = Cv ) , dt

(5.6)

Fig. 5.1. Log-log plot of vacancy and interstitial concentration vs. time for case (1) low temperature and low sink density (after [2])

5.1 Point Defect Balance Equations

with the solution: 1/2 K0 . C= Kiv Equating this concentration with that during the buildup phase: 1/2 K0 K0t = , Kiv

195

(5.7)

(5.8)

yields the time at which losses to recombination compensate for the production rate from irradiation: t = τ1 = (K0 Kiv )−1/2 ,

(5.9)

where τ1 is a time constant or characteristic time for the onset of mutual recombination. Eventually, the interstitials (first) and then the vacancies (later) will begin to find the sinks and sinks will start to contribute to annihilation. Ci and Cv remain approximately equal until a time τ2 , which is the time constant for the process of interstitials reacting with the sinks. Because Di > Dv , more interstitials are lost to sinks than vacancies, which is described by: dCi = −KisCiCs , dt

(5.10)

so the interstitial concentration will decay and the vacancy concentration will rise (since their only sink is interstitials and interstitials are being lost to sinks), yielding:

K0 KisCst 1/2 Cv (t) = Kiv (5.11)

1/2 K0 Ci (t) = . Kiv KisCst (The derivation of Eq. (5.11) is Problem 5.15 at the end of the chapter.) The time at which these equalities occur is obtained by equating the concentrations in the bounding time regimes of quasi-steady state and buildup of interstitials/decay of vacancies (Fig. 5.1): 1/2

K0 K0 KisCst 1/2 Cv = = Kiv Kiv (5.12) 1/2

1/2 K0 K0 Ci = = , Kiv Kiv KisCst and solving for the time yields the time constant for the onset of the buildup regime: t = τ2 = (KisCs )−1 .

(5.13)

196

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

After a while, at time τ3 , true steady state will be achieved. τ3 is the time constant for the slowest process, which is the interaction of vacancies with sinks. Solving Eq. (5.1) for the steady state concentration of vacancies and interstitials by setting dCv / dt = dCi / dt = 0 gives:

1/2 K 2 C2 K0 Kis KisCs + + is 2s 2Kiv Kiv Kvs 4Kiv

2 C2 1/2 KvsCs K0 Kvs Kvs s Ciss = − + + . 2Kiv Kiv Kis 4Kiv2

Cvss = −

(5.14)

Since vacancies and interstitials are produced in equal numbers and equal numbers are lost to recombination, the loss of each to sinks must be equal at steady state, and: KvsCv = KisCi .

(5.15)

For the case of low temperature and low sink density, Cs is small, and the vacancy and interstitial concentrations in Eq. (5.14) are approximated as: K0 Kis ∼ ∼ K0 Kvs . Cvss = ; Ciss = (5.16) Kiv Kvs Kiv Kis Equating these expressions to those from the previous (buildup) region gives:

Cv =

K0 KisCst Kiv

1/2 =

K0 Kis Kiv Kiv

1/2 .

(5.17)

and solving for the time gives the time constant for the onset of steady state: t = τ3 = (KvsCs )−1 .

(5.18)

The buildup shown in Fig. 5.1 is really a schematic and not the actual buildup. The transitions between regimes are not so sudden. For example, if the sink density is assumed to be zero, the exact solution to Eq. (5.1) is: "

K0 Cv (t) = tanh Kiv K0t . (5.19) Kiv 5.1.2 Case 2: Low Temperature, Intermediate Sink Density Increasing the sink density has the effect of bringing τ2 closer to τ1 (see Fig. 5.2). That is, the region of mutual recombination is shrunk at the expense of annihilation at sinks. In fact, when:

τ1 = τ2 or (K0 Kiv )−1/2 = (KisCs )−1 , the plateau disappears.

(5.20)

5.1 Point Defect Balance Equations

197

Fig. 5.2. Log-log plot of vacancy and interstitial concentration vs. time for case (2) low temperature and intermediate sink density (after [2])

5.1.3 Case 3: Low Temperature, High Sink Density The main effect of a high sink density is that interstitials find the sinks before they find vacancies because Cs Cv at short time (Fig. 5.3). That is, the time to reach linear buildup (loss of interstitials to sinks), τ2 , becomes shorter than the time to reach quasi-steady state due to vacancy–interstitial interaction, τ1 . In this case, the interstitial concentration comes into a quasi-steady state with production and annihilation at sinks: dCi = 0 = K0 − KisCiCs , (5.21) dt resulting in the quasi-steady state concentration: Ci =

K0 . KisCs

(5.22)

Equating interstitial concentrations in the linear buildup regime with the quasisteady state regime: K0t =

K0 , KisCs

(5.23)

and solving for t gives the value for the time constant τ2 : t = τ2 = (KisCs )−1 .

(5.24)

198

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.3. Log-log plot of vacancy and interstitial concentration vs. time for case (3) low temperature and high sink density (after [2])

Note that since interstitials have found the sinks before finding the slower vacancies, the vacancy concentration continues to rise according to Cv = K0 t. A competition soon arises between annihilation of interstitials at sinks and recombination with vacancies: KisCiCs = KivCiCv ∼ = KivCi K0t ,

(5.25)

yielding the time constant for the transition between the regimes where interstitials go to sinks and mutual recombination dominates: t = τ4 =

KisCs . Kiv K0

(5.26)

In the regime following τ4 , Cv rises but more slowly, and Ci decreases slowly according to: Cv = (K0 KisCs t/Kiv )1/2 Ci = (K0 /Kis KivCst)1/2 .

(5.27)

5.1 Point Defect Balance Equations

199

Steady state arrives at:

τ3 =

1 , KvsCs

(5.28)

with

1/2 Kis2 Cs2 KisCs K0 Kis =− + + 2Kiv Kiv Kvs 4Kiv2

2 C2 1/2 K0 Kvs Kvs KvsCs s Ciss = − + + . 2Kiv Kiv Kis 4Kiv2

Cvss

(5.29)

Note that the steady state concentrations are the same as Eq. (5.14) given earlier in case (1), but without the simplification of dropping the terms in Cs since in this case, the sink density is high and cannot be neglected. 5.1.4 Case 4: High Temperature At high temperature, the defect annihilation rate at the sinks keeps the concentration of interstitials low (Fig. 5.4). Since recombination does not contribute much, the rate equations become: dCv = K0 − KvsCsCv dt dCi = K0 − KisCsCi , dt

(5.30)

with steady state solutions: Cv =

K0 , KvsCs

Ci =

K0 , KisCs

(5.31)

with characteristic times given by: interstitial annihilation at sinks: vacancy annihilation at sinks:

K0 ⇒ t = τ2 = (KisCs )−1 (5.32) KisCs K0 K0t = ⇒ t = τ3 = (KvsCs )−1 . (5.33) KvsCs K0t =

The time evolution of vacancy and interstitial concentrations displayed in Fig. 5.4 ignores the presence of thermal vacancies, which may be significant at higher temperatures. The buildup of radiation-induced vacancies and interstitials at high temperature, including an initial presence of thermal equilibrium vacancies is shown in Fig. 5.5. Note the effect of sink (dislocation) density and defect production rate.

200

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.4. Log-log plot of vacancy and interstitial concentration vs. time for case (4) high temperature (after [2])

Fig. 5.5. Steady state (a) vacancy and (b) interstitial concentrations in an irradiated metal at a high production rate (solid line) and at a low defect production rate (dashed line). The upper and lower curves for each defect production rate represent small and large dislocation densities, respectively (after [3])

5.1 Point Defect Balance Equations

201

Table 5.1. Time constants for rate-limiting processes in the point defect balance equations Time constant

Value

Process

τ1 τ2 τ3

(K0 Kiv )−1/2 (KisCs )−1 (KvsCs )−1 K Cs τ12 /τ2 = is K0 Kiv

Onset of mutual recombination Onset of interstitial loss to sinks Onset of vacancy loss to sinks

τ4

Mutual recombination dominates interstitial loss to sinks

Figure 5.5a shows that increasing the sink density lowers the vacancy concentration since sinks absorb the vacancies (loss term is proportional to Kvs ). Also for a fixed sink density, a higher displacement rate results in a higher vacancy concentration because the production rate is higher than the loss rate to sinks. The same is true for interstitials shown in Fig. 5.5b. The kinks in the interstitial concentration curves correspond to the temperature at which vacancies become mobile and contribute to interstitial loss by mutual recombination as in Fig. 5.3. Comparing Figs. 5.5a,b shows that the equilibrium concentration of interstitials is negligible over the practical range of reactor component temperatures, while this is not the case for vacancies. The main objective of solving the point defect balance equations is to obtain values for Ci and Cv to determine Drad , which is just the sum of Ci Di and Cv Dv . The preceding discussion shows that we can interpret radiation-enhanced diffusion experiments after an isothermal irradiation at a constant flux for a time t in terms of characteristic times. Table 5.1 summarizes the time constants for the various ratelimiting mechanisms. For low sink density, recombination dominates at short times, followed by interstitial annihilation at sinks and then vacancy annihilation at sinks, which is the slowest process and controls the achievement of steady state. At high sink density, interstitial annihilation at sinks dominates early, followed by mutual recombination and then vacancy loss to sinks. As a rule, when τ1 < τ2 , mutual recombination dominates and when τ2 < τ1 , sinks dominate. In summary, the key factors affecting Ci and Cv are production rate, defect mobility and sink concentration. 5.1.5 Properties of the Point Defect Balance Equations The point defect balance equations and their solutions possess interesting properties, which provide further insight into the behavior of vacancies and interstitials in the diffusion of lattice atoms. They are the following: 1. The vacancy concentration referred to in the last section is really Cv −Cv0 where Cv0 is the thermal equilibrium concentration of vacancies. In high-temperature irradiations (T /Tm ≥ 0.5), this concentration is non-negligible. However, over all irradiation temperatures of interest, Ci0 /Ci 1.

202

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

2. In the absence of sinks and thermal vacancies, Cv can be exchanged with Ci , that is, Cv = Ci at any instant: dCv = K0 − KivCiCv dt dCi = K0 − KivCiCv . dt

(5.34)

Since Drad = DiCi + DvCv , and Ci = Cv , but since Di Dv , then interstitials contribute much more to atom mobility than do vacancies. 3. If there is only one type of sink, then at steady state: K0 = KivCiCv + KvsCvCs K0 = KivCiCv + KisCiCs ,

(5.35)

KvsCv = KisCi ,

(5.36)

or

and the absorption rate of interstitials and vacancies at sinks is equal, or the net absorption rate at the sink is zero. Even for the case of multiple sink types, if the sinks have the same “strength” for vacancies and interstitials, then the net flow to any sink is zero. 4. Inclusion of sink terms violates the symmetry with respect to Ci and Cv because of the different values of K (Kvs = Kis ). Symmetry is present in the steady state with regard to DiCi and DvCv (since Kis α Di and Kvs α Dv ). The physical consequence is that vacancies and interstitials contribute to atom mobility to the same extent and their actions cannot be discriminated. At steady state: 0 = K0 − KivCiCv − Kvs DvCvCs 0 = K0 − KivCiCv + Kis DiCiCs ,

(5.37)

where the K terms have been written as K = K D, giving: DvCv Kvs Cs = DiCi Kis Cs .

(5.38)

∼ K , then D C = D C which means that vacancies and interstitials So if Kvs v v i i is contribute equally to atom mobility. Even though the steady state concentration of interstitials is much lower than the steady state concentration of vacancies, they each contribute equally to atom mobility because of the faster rate of diffusion of interstitials. For any particular sink to grow, it must have a net bias for either vacancies or interstitials. In real metals, Kvs and Kis are not equal. Specific sinks have a bias for certain point defects, allowing that sink to grow. This behavior is described in more detail Sect. 5.3.

5.2 Radiation-Enhanced Diffusion

203

5.1.6 Deficiencies of the Simple Point Defect Balance Model The simple point defect model neglects numerous features of realistic systems that must be incorporated in order to obtain accurate results. For example, no account is taken for changing sink strengths, which occur as dose buildup continues due to the formation of depleted zones and defect clusters. Also, sink bias is neglected. Bias is an important factor affecting the development of the irradiated microstructure as will become evident in Chaps. 7 and 8. Defect–defect interaction and defect– impurity interaction have also been neglected. Defect–defect interaction will be important in the formation of void and interstitial loop nuclei and cannot be neglected if larger clusters are to be properly accounted for. These small clusters will serve as traps or sinks for mobile defects. In fact, vacancy clusters have been found to increase Drad in the mutual-recombination range, but are insignificant for high sink concentrations and temperatures where annealing to fixed sinks dominates [4]. Finally, the equations are unable to account for defect gradients (and in the simple form, for concentration gradients). These become very important in processes such as radiation-induced segregation (Chap. 6), in which defect fluxes give rise to concentration gradients in the alloying elements. Such processes may significantly alter the behavior of sinks and the bias of the sinks.

5.2 Radiation-Enhanced Diffusion In a pure metal, the diffusion coefficient under radiation is given by: Drad = DvCv + DiCi .

(5.39)

Because the concentrations of vacancies and interstitials under irradiation are much greater than those produced thermally, the radiation-enhanced diffusion coefficients are much larger than thermal diffusion coefficients. Despite the shortcomings, it is interesting to see how well the simple point defect balance equations are able to estimate the effect of irradiation on diffusion. Figure 5.6 is a plot of log Drad vs. logt for the case of annealed Ag-30% Zn at 40 ◦C irradiated with 2.5 MeV electrons at a flux of 3.7 ×1015 m−2 s−1 [2]. The thin solid lines are the interstitial and vacancy concentrations and the thick solid line is the their sum as calculated from Eq. (5.35) by Sizeman [2] and the dashed line is the experimental data. The experiment actually measures the Zener relaxation time, τz (see [1]), which is proportional to Drad . The experimental result confirms the existence of a maximum in Drad as in case (1) for low temperature and low sink density. This result also shows that the interstitial component dominates at times less than that to achieve steady state, τ3 , since Di > Dv (by assumption) and Ci > Cv for τ < τ3 . Another excellent example of calculation of Drad vs. measurement is provided by Rothman [5.1] for self-diffusion in copper at 200 ◦C in a crystal containing a dislocation density of 1011 m−2 under irradiation with a net damage rate,

204

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Fig. 5.6. Time dependence of Drad vs. lnt for both calculation (solid line) and measurement (dashed line). Thin solid lines are for the vacancy and interstitial components and the heavy solid line is the sum of the components (after [2])

K0 = 10−6 dpa/s (similar to that experienced by a fast reactor core structural material). In this case, Drad ∼ 6.5 ×10−21 m2 s−1 . Given that the thermal diffusion coefficient is ∼ 1.4 ×10−27 m2 s−1 , this represents an extremely large (> 106 ) increase due to irradiation. Figure 5.7 shows that at temperatures below 575 ◦C, Drad exceeds the thermal equilibrium self-diffusion coefficient for this defect production rate (curve 1). The various curves in Fig. 5.7 represent different combinations of production rates and defect densities. Note that at low temperature, mutual recomv /2 (all curves). At low bination dominates and Drad has an activation energy of Em 11 −2 sink density (10 dislocations m (curve 1), where ρd ∼ 4π rvsCs = 4π risCs ) the mutual recombination region ties indirectly to diffusion by thermal equilibrium vacancies with increasing temperature. At high sink densities, (1014 m−2 (curve 2) and 1015 m−2 (curve 3)), mutual recombination gives way to annealing at fixed sinks at a critical temperature, determined as follows. According to Eq. (5.36), for a single sink type: Ci Kis = Cv Kvs

or Ci =

Cv Kvs . Kis

(5.40)

5.2 Radiation-Enhanced Diffusion

205

Fig. 5.7. Calculated Drad for self-diffusion of copper as a function of temperature for different combinations of defect production rates and dislocation densities. 1: K0 = 10−6 dpa/s, ρd = 1011 m−2 , 2: K0 = 10−6 dpa/s, ρd = 1014 m−2 , 3: K0 = 10−6 dpa/s, ρd = 1015 m−2 , 4: K0 = 10−4 dpa/s, ρd = 1011 m−2 (after [1])

At steady state, Eq. (5.29) apply and they can be re-written in the following form: KisCs 4K0 Kiv 1/2 Cv = −1 1+ 2Kiv Kis KvsCs2 (5.41) KvsCs 4K0 Kiv 1/2 Ci = −1 . 1+ 2Kiv Kis KvsCs2 We define a parameter, η , such that:

η=

4K0 Kiv . Kvs KivCs2

(5.42)

Then using Eq. (5.41) Cv can be written as: Cv =

F(η )K0 , or Cv KvsCs = F(η )K0 . KvsCs

(5.43)

where: F(η ) =

2 [(1 + η )1/2 − 1] . η

(5.44)

Equation (5.43) shows that F(η ) determines the number of defects absorbed by sinks in relation to the total rate of formation of the defects. If η → 0, then

206

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

F(η ) → 1, i.e., all of the defects are lost to sinks and none to recombination. In the limit of large η , F(η ) ∼ 2/η 1/2 and F(η ) → 0, indicating that mutual recombination dominates defect loss. When F(η ) = 1/2, the loss of defects to sinks and recombination is equal. This occurs at a value of η of:

η =8=

4K0 Kiv . Kvs KisCs2

(5.45)

Equation (5.45) can be solved for the critical temperature below which mutual recombination will dominate, and above which loss to sinks will dominate. (The term η will be revisited in Chap. 8 in describing the effect of recombination on void growth). Using Eqs. (5.3), (5.4), and (5.5) for Kiv , Kis and Kvs , and defining = 4π r , gives: Kiv = 4π riv , Kis = 4π rvs and Kvs iv i −Em 4K0 Kiv Di0 exp kT 8= , (5.46) v i −Em Di exp −Em C2 Dv exp Kvs K s 0 is 0 kT kT v is the migration energy and Di,v is the pre-exponential factor in the difwhere Ei,m 0 fusion coefficient for interstitials and vacancies, respectively. Equation (5.46) simplifies to:

Tc =

k ln

v Em v 2D0Cs2 Kis Kvs K0 Kiv

.

(5.47)

At the highest temperatures, Drad is overwhelmed by thermal vacancies (all curves in Fig. 5.7), and increasing K0 to 10−4 dpa/s (curve 4) raises Drad in the mutual recombination range by a factor of 10. Figure 5.8 shows the radiation-enhanced diffusion coefficient calculated for a sample of nickel undergoing irradiation at a rate of 10−6 dpa/s for different sink annihilation probabilities, p, where p−1 is the average number of jumps of a defect between creation and annihilation at a sink [5]. The diffusion coefficient describing radiation-enhanced diffusion, Drad , is shown by the solid line. The dashed line to the left is the thermal diffusion coefficient and the solid horizontal line at the right is the diffusion coefficient due to ballistic mixing, Dm [6], and will be discussed in Chap. 10. The difference between the curves for Drad and Dth is the effect of radiation-enhanced diffusion. As shown, irradiation can result in a several orders of magnitude increase in the diffusion coefficient.

5.3 Defect Reactions Each of the terms in the point defect balance equation represents a reaction. The rate at which the reaction occurs will depend on the nature of the reacting species.

5.3 Defect Reactions

207

Fig. 5.8. Diffusion coefficient as a function of 1/T for a nickel-base alloy during irradiation at a displacement rate of 10−6 dpa/s. Drad is calculated from rate theory for various sink annihilation probabilities, p. The diffusion coefficient from displacement mixing is Dm and the thermal diffusion coefficient is Dth (from [5])

Following [3], we will develop expressions for the rates of each of the reactions in the point defect balance equation, as they will be used in describing processes such as void growth, dislocation climb, etc. We have seen that the motion of mobile point defects can be considered a random walk process. When one of these defects encounters a specie in the crystal to which it becomes tightly bound, one or both of the partners in the encounter is considered to disappear from the solid. Examples include a vacancy or interstitial intersecting a free surface, grain boundary, dislocation, void, etc., or a vacancy encountering a vacancy, an interstitial encountering an interstitial, or a vacancy encountering an interstitial. Clearly the rate of such reactions is proportional to the concentrations of both species, or: reaction rate of A and B = KABCACB reactions/cm3 s ,

(5.48)

where CA and CB are the concentration of species A and B in units of particles/cm3, and KAB is the rate constant of the reaction in cm3 /s. Reactions can be between two mobile particles (vacancy and interstitial at high temperature) or between one mobile and one stationary defect, e.g., low temperature where vacancies are immobile and interstitials are mobile, or between interstitials and dislocation, grain boundaries, voids, etc. There are two types of processes that will be of interest in dealing with the reaction between point defects and sinks. They are reaction rate-controlled and diffusion-controlled processes. In reaction rate-governed processes, there must be no macroscopic concentration gradients of either partner. If one partner is large compared to the atomic sized reactant, or if one is a strong sink, a concentration gradient may be established in the vicinity of the stationary defect. Reactions between point defects are examples of reaction rate-controlled processes. If a defect

208

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory Fig. 5.9. Locations of nearest neighbors for the formation of a di-vacancy in the fcc lattice (after [3])

concentration gradient is established, the overall process is governed by the rate of diffusion of the mobile species to the stationary sink. This is the case with free surfaces, voids and grain boundaries. These defects are usually not treated by reaction rate theory. As a first example of a reaction rate-controlled process, let us look at the vacancy–vacancy reaction. Consider the reaction: v + v → v2 ,

(5.49)

that proceeds in the forward direction only and is characterized by the rate constant K2v . In this example, one vacancy is assumed to be stationary and the other is mobile. The rate of di-vacancy formation per cm3 is: R2v = P2vCv

(5.50)

where Cv is the concentration of monovacancies and P2v is the probability per second that another vacancy jumps into a site that is a nearest neighbor to a particular vacancy (Fig. 5.9). A di-vacancy will form if a nearest neighbor site to a vacancy is occupied by another vacancy, thus P2v depends on the crystal structure. Taking the fcc lattice, all 12 nearest neighbor sites are equivalent, yielding: P2v = 12Px ,

(5.51)

where Px is the probability per second that another vacancy jumps into one of the nearest neighbor positions surrounding the vacancy. Px is proportional to: 1. The number of sites surrounding the nearest neighbor site from which another vacancy could jump (seven sites as shown by the dashed atoms in Fig. 5.9)

5.3 Defect Reactions

209

2. The probability that one of these lattice positions is occupied by a vacancy, Nv 3. The jump frequency of a vacancy, ω , or Px = 7Nv ωv ,

(5.52)

and we can write the vacancy site fraction as Nv = Cv Ω , where Cv is the volumetric vacancy concentration and Ω is the atomic volume. Back substitution of Eqs. (5.51) and (5.52) into Eq. (5.50) yields: R2v = 84ωΩ Cv2 [cm−3 s−1 ] .

(5.53)

Comparison with the definition of the reaction rate, Eq. (5.48) gives the reaction rate constant K2v : K2v = 84ωΩ .

(5.54)

In the fcc lattice, Dv = a2 ω , then K2v =

84Ω Dv . a2

(5.55)

Although the expression for the rate constant was derived for a vacancy–vacancy reaction, the same formulation applies to any reaction between any specie (e.g., impurity) that occupies substitutional positions in the fcc lattice. It can also be used for other lattice types, but the factor, 84, called the combinatorial factor is dependent on the crystal structure. The combinatorial factor is the solid state analog of the cross section in particle interactions. In the previous example, we forced one of the reactants to be stationary. When the reaction is between two mobile species, the rate is (KAB + KBA )CACB , where KAB is the rate constant calculated assuming that B is immobile and vice versa for KBA . Therefore, if both vacancies are mobile, the result would be multiplied by a factor of 2; K2v + K2v = 2K2v . Given this background, we now turn our attention to the various terms in the point defect balance equations in order to develop expressions for the reaction rate coefficients. 5.3.1 Defect Production The first term in the defect balance equations of Eq. (5.1) is the production rate of vacancies and interstitials and this was determined in Chap. 2, Eq. (2.125), where the term in brackets is given the designation, FP : K0 = ξ νFP σs N φ [cm−3 s−1 ] .

(5.56)

For stainless steel, νFP ∼ 30 Frenkel pairs per collision, σs ∼ 3 ×10−24 cm2 and N ∼ 7 ×1022 cm−3 . The term, ξ , is the displacement efficiency (Chap. 3) that accounts for the reduction in freely migrating point defects due to in-cascade recombination and clustering.

210

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.3.2 Recombination The second term in Eq. (5.1), KivCvCi is the recombination rate. The rate constant Kiv is the same for both vacancies and interstitials since they must recombine with each other at the same rate. Reactions between vacancies and interstitials are of great importance since the result is mutual annihilation or return to the perfect lattice. Assuming a stationary vacancy and a mobile interstitial, and that recombination only occurs when the interstitial jumps into a site that is nearest neighbor to the vacancy, we can determine the recombination rate constant for an octahedral interstitial in the fcc lattice. There are six octahedral sites as nearest neighbors to the vacant lattice site and each lattice site has eight octahedral nearest neighbors, giving a value of 48 for the combinatorial factor: Kiv =

48Ω Di . a2

(5.57)

However, this is a bit unrealistic since (1) the stable form of the interstitial is the split interstitial, and (2) the vacancy and interstitial are attracted to each other by virtue of their strain fields, causing spontaneous recombination to occur over distances greater than the nearest neighbor spacing. Therefore, a more realistic estimate of the combinatorial factor, ziv is ∼ 500: Kiv =

ziv Ω Di , and ziv ∼ 500 . a2

(5.58)

5.3.3 Loss to Sinks The loss term represents all the possible sinks for vacancy and interstitial loss. These sinks can be divided into three categories: 1. Neutral (unbiased) sinks show no preference for capturing one type of defect over the other type. The rate of absorption is proportional to the product of the diffusion coefficient of the point defect and the difference in the concentrations of the point defect in the bulk metal and at the sink surface. The types of sinks in this category are voids, incoherent precipitates and grain boundaries. 2. Biased sinks exhibit preferential attraction for one defect type over the other. Dislocations exhibit a stronger preference for interstitials than for vacancies. The bias is due to the drift of interstitials down the stress gradient near the dislocation core. Since absorption of interstitials enhances dislocation climb, the dislocation is an unsaturable sink. Two types of dislocations are considered; networks in unirradiated metal and from unfaulted Frank loops, and interstitial dislocation loops. 3. Variable bias sinks such as coherent precipitates act as traps, which capture a defect but preserve its identity until it is annihilated by the opposite type defect. Impurity atoms and coherent precipitates act as recombination centers with a limited capacity.

5.4 Reaction Rate-Controlled Processes

211

5.3.4 Sink Strengths Reaction rate constants describe the reaction and are designated a point defect and a sink (which may be another point defect), and are designated K jX where j is the mobile point defect and X is the sink. As such, they include the diffusion coefficient of the point defect as well as a description of the tendency for the reaction to occur. It is often useful to describe the tendency of a sink to absorb defects that is independent of the defect properties. The sink strength, with units of cm−2 , is such a description and it reflects the strength or affinity of a sink for defects. Sink strength is independent of defect properties for neutral sinks. The sink strength is defined as: absorption rate = K jX C jCX = k2jX C j D j ,

(5.59)

so K jX CX , Dj

k2jX =

(5.60)

or k2j = ∑ k2jX .

(5.61)

X

Both the rate constant and the sink strength are terms commonly used to describe the action of sinks on the defects in the solid. Physically, k−1 j is the mean distance a free defect of type j travels in the solid before becoming trapped. Before we treat the various sink types, we will first look at the rate constants for the two basic reaction processes; reaction rate-controlled processes and diffusionlimited processes. We begin with reaction rate-controlled processes.

5.4 Reaction Rate-Controlled Processes 5.4.1 Defect–Void Interaction For reactions where capture is controlled by the rate at which the point defects enter the trap site, we can use Eq. (5.58). For defect–void reactions, the term to be determined is the combinatorial factor. For a void, the number of lattice points on the surface of the sphere is 4π R2/a2 , where the area occupied by a lattice point is approximated at a2 . The rate constant then becomes: KvV =

4 π R 2 Ω Dv 4 π R 2 Dv , = a4 a

2 where Ω ∼ a3 , kV =

where ρV is the concentration of voids in the solid.

4 π R2 ρ V , a

(5.62)

212

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.4.2 Defect–Dislocation Interaction Consider a cylinder about a dislocation line whose axis is coincident with the dislocation line such that capture is certain for any vacancy entering the cylinder (Fig. 5.10). The cylinder consists of zvd atomic sites on each of the crystal planes intersected by the dislocation line. The cylinder defines the capture radius of the dislocation, or the radius inside which entering defects are lost to the sink. If the spacing between atom planes in the lattice is ∼ a, then there are zvd /a capture sites per unit length of dislocation. Letting ρd be the density of dislocation lines in the crystal (in units of centimeters of dislocation line per cm3 of solid or cm−2 ), then there are zvd ρd /a capture sites per unit volume. If the concentration of vacancies per unit volume is Cv , then the vacancy site fraction is Cv Ω . For a vacancy jump rate of ω , the rate of vacancy capture rate by the dislocation per cm3 is: Rvd =

zvd ρd Cv Ω ω [cm−3 s−1 ] . a

(5.63)

Since Ω ∼ a3 and Dv = a2 ω , we have: 2 = zvd ρd Rvd = Dv zvd ρdCv and reaction rate constant Kvd = Dv zvd , kvd 2 Rid = Di zid ρdCi and reaction rate constant Kid = Di zid , kid = zid ρd

(5.64)

and zvd = zid .

5.5 Diffusion-Limited Reactions Reactions between defects and sinks cannot always be characterized as reaction ratelimited. Reactions driven by defect concentration gradients are diffusion-limited and must be treated differently. Such reactions are defect–void, defect–grain boundary and sometimes defect–dislocation interactions. Following [3], these reactions are addressed here starting with defect–void reactions.

Fig. 5.10. Capture volume around a dislocation line, defined by the cylinder of radius Rd and with sink sites lying on crystal planes separated by a distance a

5.5 Diffusion-Limited Reactions

213

5.5.1 Defect–Void Reactions Consider the case of ρV voids per unit volume, each of radius, R, which absorb a particular type of point defect present in the solid and between the spherical sinks. Focusing on a single sphere, the unit cell or capture volume surrounding each sphere is defined as the portion of the solid that can be associated with each sphere. The radius of the capture volume (see Fig. 5.11) around each sphere is defined by: 4 π R3 ρV = 1 . (5.65) 3 The diffusion equation for the point defects will be solved in the spherical shell R ≤ r ≤ R. The concentration of point defects at a radial position r in the capture volume at time t is denoted by C(r,t). The definition of the capture volume implies that there is no net flux of point defects across the boundary at r = R which is written as: ∂C =0, (5.66) ∂r R and the point defect concentration at the surface of the sphere is: C(R,t) = CR .

(5.67)

The value of CR depends on the process. For insoluble gas atoms where the spheres represent gas bubbles, CR = 0. For bubbles or voids where the point defects are 0 , the thermal equilibrium defect concentration. vacancies or interstitials, CR = Cv,i If the defects are created uniformly in the capture volume and no sinks other than the sphere are present, then the concentration C(r,t) is determined by solution of the volumetric diffusion equation with a volumetric source term: D ∂ ∂C ∂C = 2 (5.68) r2 + K0 , ∂t r ∂r dr where D is the diffusion coefficient of the defects (assumed to be independent of concentration) and K0 is the defect production rate per unit volume given by Eq. (5.56).

Fig. 5.11. The unit cell for determination of the diffusion-controlled rate constant for defect absorption by a spherical sink

214

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

When a solid is irradiated at a temperature where point defects are mobile, the loss of particles to the sink is partially compensated by the production rate so the ∂C ∼ 0 and Eq. (5.61) can be approxiconcentration changes slowly with time ∂t mated as: D d 2 dC (5.69) r = −K0 . r2 dr dr The solution to Eq. (5.69) subject to the boundary conditions given by Eqs. (5.66) and (5.67) is:

K0 2R2 (r − R) 2 C(r) = CR + − r − R2 . (5.70) 6D rR Since in many cases, the capture volume radius is much larger than the sink radius and the defect concentration changes rapidly only very close to the sink, the capture volume is divided into two regions (Fig. 5.12). In region 1 the diffusion term is much greater than the source term and Eq. (5.69) can be approximated by: 1 d 2 dC r =0, (5.71) r2 dr dr with boundary conditions: C(R) = CR

(5.72)

C(∞) = C(R) .

(5.73)

The solution of Eq. (5.71) subject to the boundary conditions given by Eqs. (5.72) and (5.73) gives:

R C(r) = CR + [C(R) − CR ] 1 − . (5.74) r The flux of particles at the void surface is defined by: dC . J = −D dr R

(5.75)

Using Eq. (5.70) gives: J=

−D[C(R) − CR ] . R

(5.76)

The absorption rate of point defects by the void is: −(4π R2)J = 4π RD[C(R) − CR] .

(5.77)

Requiring that point defects produced in the capture volume be absorbed by the void gives: 4 π (R3 − R3)K0 = 4π RD[C(R) − CR ] . 3

(5.78)

5.5 Diffusion-Limited Reactions

215

Fig. 5.12. Regions of interest in the solution of the diffusion equation in a spherical shell with a uniform volumetric production rate of defects

If R3 R3 , the balance becomes: C(R) = CR +

K0 R3 . 3RD

(5.79)

Assuming that C(R) CR in Eq. (5.56) and replacing C(R) by C, we obtain the total rate of diffusion-controlled absorption of point defects by the void by multiplying Eq. (5.77) by the number of voids per unit volume ρV : Rate of absorption/cm3 = 4π RDρVC .

(5.80)

The rate constant for diffusion-controlled reaction of point defects and a perfect spherical sink of radius R is then: KiV = 4π RDi , KvV = 4π RDv , 2 = 4 π Rρ V , kV

(5.81)

where the subscripts of K refer to the reacting species, vacancies or interstitials (v, i) and voids, V . 5.5.2 Defect–Dislocation Reactions Diffusion-controlled reactions between defects and dislocations occur in much the same way as in the case of spherical sinks, but in cylindrical coordinates. Taking the capture radius of the sink to be Rd and the dislocation density to be ρd , we define the unit cell such that: (π R2 )ρd = 1 . The diffusion equation is: D d dC r + K0 = 1 r dr dr

(5.82)

(5.83)

216

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

with boundary conditions:

C(Rd ) = CRd dC =0, dr R

(5.84) (5.85)

and solution: C(r) = CRd +

2

r − R2d K0 R2 r − 1/2 . ln 2D Rd R2

(5.86)

Analogous to the case for spherical sinks, in region 1, but in cylindrical geometry instead, the diffusion equation is: dC 1 d r =0, (5.87) r dr dr with boundary conditions: C(Rd ) = CRd C(R) = C ,

(5.88) (5.89)

with solution: C(r) = CRd + [C(R) − CRd ]

ln(r/Rd ) . ln(R/Rd )

The flux of defects to the dislocation line is: −D[C(R) − CRd ] dC . = J = −D dr Rd Rd ln(R/Rd )

(5.90)

(5.91)

The absorption rate per unit length of dislocation line = −(2π Rd)J =

2π D[C(R) − CRd ] . ln(R/Rd )

(5.92)

The rate of defect production in the capture volume = π (R2 − R2d )K0 ,

(5.93)

and since all defects produced in the capture volume are captured by the dislocation: 2π D[C(R) − CRd ] = π (R2 − R2d)K0 , ln(R/Rd )

(5.94)

and C(R) = CRd +

K0 R2 ln(R/Rd ) for Rd /R 1 , 2D

(5.95)

5.6 Mixed Rate Control

217

so from Eq. (5.91) the rate of defect capture by dislocations per unit volume = 2π DρdC , and the rate constants for vacancies and interstitials are: ln(R/Rd ) 2 π Dv ln(R/Rvd ) 2 π Di , Kid = ln(R/Rid )

(5.96)

2πρd ln(R/Rvd ) 2πρd 2 . = kid ln(R/Rid )

(5.97)

Kvd =

and 2 kvd =

Note that the combinatorial factors for vacancies and interstitials differ by the capture radius. The capture radius for interstitials is slightly greater than that for vacancies and is the origin of the dislocation bias for interstitials.

5.6 Mixed Rate Control Mixed rate control occurs when the reaction rate is determined by a combination of processes. We can determine the rate constant for the combined processes by adding the reciprocals of the rate constants to give the resistance due to series steps of diffusion and surface attachment. For the case of voids, we use the rate constants given by Eqs. (5.62) and (5.81), and: 1 1 1 = + , Keff Kreaction Kdiffusion

(5.98)

to yield the effective rate constant: Keff =

4π RD a , 1+ R

2 = keff

4 π Rρ V a . 1+ R

(5.99)

For large spheres, a/R → 0 and the rate constant is that for diffusion only. This result shows that reaction rate limitations to capture kinetics for spherical sinks are only significant if the sphere radius is small, approaching the lattice constant. For dislocations, the capture rates calculated from a diffusion-controlled process vs. a reaction rate-controlled process are: 2π D ln(R/Rd ) Kreaction = zd D ,

Kdiffusion =

(5.100)

218

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

giving the effective rate constant for mixed-control: Keff =

D , 1 ln(R/Rd ) + zd 2π

2 keff =

ρd . 1 ln(R/Rd ) + zd 2π

(5.101)

Consider zd to be the area of a circular region of radius Rd divided by the number of atoms per unit area. For the (100) plane of the fcc lattice, the number of atoms/unit area is 2/a2 a/cm2 and: Kreaction /D = zd /D =

2π R2d = 24 for Rd ∼ 0.6 nm and a ∼ 0.3 nm . a2

For a dislocation line density of 1010 cm−2 , Kdiffusion /D = ture of defects by dislocations is diffusion-controlled.

(5.102)

2π = 1.4. So capln(R/Rd )

5.7 Defect–Grain Boundary Reactions Interactions between point defects and grain boundaries are important in the case of radiation-induced segregation, discussed in Chap. 6. Following the analysis of Heald and Harbottle [7], the sink strength of the grain boundary is determined by considering a spherical grain of radius a, with grain boundary defect concentration equal to the thermal equilibrium value, which will be neglected compared to the irradiated-induced concentration. The loss to sinks within the grain is: k2 DC = (zd ρd + 4π RVρV )DC ,

(5.103)

where k2 is the sink strength for the grain interior due to dislocations and voids, and the diffusion equation is: d2C 2 dC K0 + − k 2C = 0 , + dr2 r dr D

(5.104)

subject to boundary conditions C(r = a) = 0 and C(r = 0) = finite. The solution to Eq. (5.104) subject to the boundary conditions is:

K0 a sinh(kr) C(r) = 1− , (5.105) Dk2 r sinh(ka) and the total flow of point defects to the grain boundary, A is: 4π K0 a ∂ C = [ka cot(ka) − 1] . A = −4π r2D ∂ r r=a k2

(5.106)

5.8 Coherent Precipitates and Solutes

219

Written in rate theory formalism, Eq. (5.106) becomes: A = zgb DC0 ,

(5.107)

where zgb is the sink strength for an individual grain boundary and C0 is the concentration at the grain center (r = 0):

ka K0 1− C0 = C(r = 0) = . (5.108) Dk2 sinh(ka) From Eqs. (5.106), (5.107), and (5.108), the grain boundary sink strength, zgb is

ka cosh(ka) − sinh(ka) zgb = 4π a . (5.109) sinh(ka) − ka For small grains and low sink strengths, ka → 0, and: zgb (ka → 0) = 8π a = 4π d ,

(5.110)

where d(= 2a) is the grain diameter. When sink strength is large, ka → ∞, and: zgb (ka → ∞) = 4π ka2 = π kd 2 .

(5.111)

The grain boundary sink strength is the product of zgb and the grain density in grains per unit volume, or ρgb = 6/π d 3, giving: 2 kgb (ka → 0) = 24/d 2 ,

K jgb = 4π D j d ,

(5.112)

2 (ka → ∞) = 6k/d , kgb

K jgb = π kD j d 2 ,

(5.113)

and

where j = i or v. Generally, k2 ∼ 1011 cm−2 and d > 10−3 cm so that Eq. (5.113) is the appropriate expression for the grain boundary sink strength. In fact, the grain boundary sink strength is given by Eq. (5.113) whenever (zd ρd + 4π RVρV ) > 1/d.

5.8 Coherent Precipitates and Solutes These types of sinks are known as variable bias sinks in that they act as traps for vacancies and interstitials rather than as infinite sinks in which the defect loses its identity after being absorbed. The source of the attraction of vacancies and interstitials to the trap is the relief of the strain field produced by the coherency between the trap and the lattice. The coherent precipitate is of a structure in which the lattice planes of the precipitate are continuous with those of the matrix, but due to the difference in lattice parameters, there is a strain field at the interface where the lattice planes from each are forced to match. The over- or undersized solute is a limiting

220

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory Fig. 5.13. Diffusion-controlled reaction between vacancies and a grain boundary

case of a coherent precipitate. The trap strength is limited by the capacity of the interface to hold or trap a defect until the anti-defect arrives and results in annihilation. Hence, no matter accumulates at this defect and thermal emission does not occur. The interface does exhibit a bias for defects and this bias is a function of the biased sinks in the solid. For example, if the biased sinks in the solid favor interstitials, then ki2 > kv2 and the trap interface will acquire slightly more vacancies than interstitials. This excess of vacancies then causes the trap surface to become a more effective sink for interstitials than for vacancies. The biases for the trap are denoted by Yv and Yi (Brailsford and Bullough [8] and Olander [3] provide detailed analyses of the bias factors), and the absorption rates of vacancies and interstitials at the trap is given by: ACP v = 4π RCPDvCv ρCPYv = KvCPCv ρCP ACP i = 4π RCPDiCi ρCPYi = KiCPCi ρCP .

(5.114)

If there can be no steady state accumulation of defects at the trap, then there is no net matter flow to or from the sinks and: 4π RCP ρCPCvYv = 4π RCP ρCPCiYi ,

(5.115)

so Yi =

DvCv Yv , DiCi

(5.116)

and the rate constants and sink strengths are: KvCP = 4π RCP DvYv ;

2 kvCP = 4π RCP ρCPYv

KiCP = 4π RCP DiYi ;

2 kiCP = 4π RCPρCPYi .

(5.117)

So variable bias sinks play an interesting role in that they adjust their preference for point defects in response to the relative sink strengths in the bulk. The reaction rate constants for the various reactions are summarized in Table 5.2 for the various defect–defect, and defect–sink reactions.

v,i + coherent ppt

Diffusion control

v,i + grain boundary

Mixed rate control

Reaction rate control

Diffusion control

v,i + dislocation

Mixed rate control

Diffusion control

Reaction rate control

v,i + void

v+i

i+i

v+v

Reaction

Di = ln(R/Rid ) 1 + zid 2π

KiCP = 4π RCP DiYi

2 kigb = Di d 4 3 Kigb = 6kDi d 5

KvCP = 4π RCP DvYv ,

2 kvgb = Dv d 4 3 Kvgb = 6kDv d 5

2π Di ln(R/Rid )

= zid Di

Kid =

Dv = ln(R/Rvd ) 1 + zvd 2π

= zvd Dv

Kvd =

2π Dv ln(R/Rvd )

4π RDi a 1+ R

=

4π RDv a 1+ R

=

4π R2 Di a = 4π RDi

KiV =

4π R2 Dv a = 4π RDv

KvV =

K2v =

z2v Ω Dv a2 z2i Ω Di K2i = a2 ziv Ω Di Kiv = a2

Rate constant

Table 5.2. Reaction rate constants for defect–sink reactions

2πρd ln(R/Rvd )

4π RρV a 1+ R 2 = kid

> 10−3 cm

= 4π RCP ρCPYv ,

= 6k/d, d 2 kvCP

2 kgb

2πρd ln(R/Rid )

= 4π RCP ρCPYi

ρd = ln(R/Rid ) 1 + zid 2π

= zid ρd

2 kiCP

2 = 24/d 2 , d < 10−3 cm kgb

ρd = ln(R/Rvd ) 1 + zvd 2π

= zvd ρd

2 = kvd

=

2 = kV

Eq. (5.117)

Eq. (5.113)

Eq. (5.112)

Eq. (5.101)

Eq. (5.64)

Eqs. (5.96), (5.97)

Eq. (5.99)

Eq. (5.81)

Eq. (5.62)

Eq. (5.58)

Eq. (5.55)

– –

Eq. (5.55)

Eq. #

–

4π R2 ρV a = 4π RρV

Sink strength

5.8 Coherent Precipitates and Solutes 221

222

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

Nomenclature A a C Civ CR Cs D Drad Dth Dm Dy0 y Dx y Em f i v s Jx k kX2 K0 Kgb Kid Kiv Kis Kvd Kvs K2v N riv ris rvs p P2v Px Rd Rid Rvd R2v

Flow rate of defects to sink Lattice constant, grain radius Concentration Interstitial, vacancy concentration Vacancy concentration at void boundary Sink concentration Grain diameter Radiation enhanced diffusion coefficient Thermal diffusion coefficient Ballistic mixing diffusion coefficient Pre-exponential factor in the diffusion coefficient via defect y Diffusion coefficient for species x via y Migration energy of defect y Correlation coefficient Interstitial designation Vacancy designation Sink designation Flux of atom or defect x across a marker plane Boltzmann’s constant Sink strength of sink X Defect production rate Rate constant for defect–grain boundary interaction Rate constant for interstitial–dislocation interaction Vacancy–interstitial recombination rate constant Interstitial–sink reaction rate constant Rate constant for vacancy–dislocation interaction Vacancy–sink reaction rate constant Di-vacancy formation rate constant Atom fraction Vacancy–interstitial recombination radius Interstitial–sink recombination radius Vacancy–sink recombination radius Sink annihilation probability Probability/second of forming a di-vacancy Probability/second that a vacancy jumps to a nearest neighbor to a vacancy Dislocation core radius Reaction rate between interstitials and dislocations Reaction rate between vacancies and dislocations Rate of di-vacancy formation

Problems

R t T Tc ν2 zgb zxy

Radius of unit cell or capture volume surrounding a spherical sink Time Temperature Critical temperature defined by Eq. (5.47) Di-vacancy designation Sink strength for an individual grain boundary Combinatorial number for a reaction between x and y

φ ρd η σs τx ω Ω ξ

Particle flux Dislocation density Parameter defined by Eq. (5.45) Microscopic scattering cross section Time constant for process x Jump frequency Atomic volume Production efficiency term

223

Subscripts a CP d gb i, v m rad R s V

Atoms Coherent precipitate Dislocation Grain boundary Interstitials, vacancies Migration Under irradiation Void radius Sink Void

Superscripts i, v

Interstitials, vacancies

Problems 5.1 Point defect concentration build up during irradiation can be described by: dCv = K0 − KivCiCv − KvsCvCs + ∇ · (Dv ∇Cv ) dt dCi = K0 − KivCiCv − KisCiCs + ∇ · (Di ∇Ci ) dt How do these equations simplify if you are irradiating a single crystal with no defects present? In that case, what is the relationship between vacancy and interstitial concentrations? Do the vacancy and interstitial concentrations differ if you start with a sample that contains defects?

224

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

5.2 For pure nickel irradiated at 500 ◦C: a) calculate the steady state concentration of vacancies and interstitials. K0 = 5 ×10−4 dpa/s

ΔHmv = 0.82 eV

Cs = 109 cm−3

ΔHmi = 0.12 eV

v i riv = ris = rvs = 10a ΔSm = ΔSm =0

ν = 1013 s−1 b) for a dislocation density of 1012 cm−2 , determine the temperature at which mutual recombination gives way to annealing at fixed sinks. 5.3 A perfect, single crystal Cu wire (cylinder) of radius R = 10 nm and length L R is irradiated at 400 ◦C. The only sink present is the surface. a) Assuming negligible recombination, solve the diffusion equation

∂ Cx = K0 + Dx ∇2Cx ∂t at steady state for x = interstitial or vacancy, to obtain the vacancy and interstitial concentration profiles. What boundary condition do you use at the surface? When you solve the equation, pay attention to the symmetry of the problem to eliminate terms in the expression for ∇2Cx . b) Calculate the rates of absorption (number of defects per unit area and time) at the surface. (Hint: remember that ∇2C is continuous.) 5.4 Calculate the steady state radiation-enhanced diffusion coefficient for copper at T /Tm = 0.5 in terms of K0 , the defect production rate, and ρd , the dislocation sink density. 5.5 Assume for a metal of interest that the interstitial–sink interaction radius and the vacancy–sink interaction radius are equal. Two irradiations are performed at low, but non-negligible sink density. The displacement rate is the same for both irradiations. In the second irradiation, a minor alloying addition doubles the diffusion coefficient of interstitials but does not change the diffusion coefficient for vacancies. By how much does the ratio of the steady state vacancy to interstitial concentrations change? Explain physically what happens to the point defects. 5.6 A sample of aluminum is held at room temperature (20 ◦C) and irradiated with a monoenergetic beam of 1 MeV neutrons at a flux of 1014 n/cm2 s. Assume that the capture radii riv = ris = rvs are all approximately 10a. a) At what sink density does defect annihilation at sinks overtake mutual recombination? b) What is the value of the radiation-enhanced steady state diffusion coefficient of aluminum atoms? How does this compare to the diffusion coefficient in the absence of irradiation? c) Verify that your calculations in part (b) do indeed represent a steady state condition, i.e., dCv / dt = dCi / dt = 0.

Problems

225

5.7 A defect-free Al crystal is irradiated at a displacement rate of 10−5 dpa/s. a) Calculate the steady state concentration of point defects at T = 100 ◦C and 500 ◦C. b) Once steady state is reached, the irradiation is stopped. Calculate the time constant for recombination as a function of temperature. c) One wishes to measure the defect concentration in the irradiated Al, a process assumed to take 100 s. Determine the temperature range for which the defect concentration can be kept within 1% of its value at the end of the irradiation for this length of time. Assume the combinatorial factor, z = 500. 5.8 Following the analysis for the diffusion rate of point defects to spherical sinks, derive an expression for the vacancy concentration profile around a dislocation. What is the vacancy capture rate by dislocations? 5.9 For fcc nickel, determine whether vacancy capture by dislocations is a diffusion-controlled or reaction rate-controlled process. What about interstitial capture by dislocations? zd = Area of the circular region about the dislocation (defined by the capture radius) divided by the number of atoms per unit area rvd = Capture radius for vacancies = 0.6 nm rid = Capture radius for interstitials = 0.7 nm 5.10 It can be shown that the time constant (characteristic time) for the process v+ s → s is t3 = (KvsCs )−1 . At sufficiently high temperature, vacancies may be sufficiently mobile so that the reaction v + v → v2 may terminate the increase in vacancy concentration with time. If the consumption rate of vacancies in di-vacancy formation is KvvCv2 , determine the time constant for the onset of steady state. 5.11 A sample of fcc copper with a low sink density (τ1 < τ2 ) is irradiated at low temperature (T /Tm = 0.3) until steady state is reached. Some time later, all sinks instantly disappear and a new steady state is reached. Determine the magnitude of the change in Cv and Ci between the two steady states. 5.12 Explain the reason (or likely reasons) for the following observations: a) The displacement rate at the surface of a copper sample is 1000 times higher when irradiated with 1 MeV Cu+ ions than with 1 MeV protons at the same flux. b) A scattering experiment using 3 MeV B+ ions on Cu produces yields that disagree sharply with calculations using the Rutherford scattering formula. Why? c) A single crystal of copper is irradiated with 2 MeV He+ ions and the backscatter yield is only 5% of that of a polycrystal. d) Irradiation of a metal with a high neutron flux does not produce a measurable increase in the atom diffusion coefficient. e) Two metals are pressed together and heated to 0.5Tm. It is observed that atoms from the metals intermix at the interface. Attempts to determine the

226

5 Radiation-Enhanced and Diffusion Defect Reaction Rate Theory

defect(s) responsible for the intermixing reveal that vacancies account for 100% of the atom mixing. True or false? Why? 5.13 Two engineers are arguing over how to test the effect of the high point defect concentration developed during irradiation on the deformation rate of nickel at 500 ◦C. Engineer #1 maintains that one can irradiate the sample to the appropriate fluence at the temperature of interest, remove it from the reactor, and heat it back up to temperature to perform the test. Engineer #2 insists that the concentration of point defects decays almost immediately after irradiation ceases and therefore, tests must be performed in situ. Who is right? Why? (Hint: consider the point defect equation for the slowest defect (vacancy) only neglect recombination and consider that the only sinks present are dislocations at a concentration of 109 cm−2 ). ◦ −8 2 DNi v (500 C) ∼ 10 cm /s

a ∼ 0.3 nm 5.14 Assume a solid containing defect sinks is irradiated at a temperature T0 , at which only vacancies are mobile. a) For the case of a high sink density, estimate the time, t1 at which sinks will contribute to vacancy annihilation. Neglect recombination. b) For the case of a low sink density, estimate the time, t2 at which recombination will contribute to vacancy annihilation. Neglect the effect of sinks. c) Describe what changes can be made in either the irradiation process or the material microstructure to force t1 = t2 . Assume a quasi-steady state condition exists, beginning at t1 in part (a) and at t2 in part (b). 5.15 Show that, for a metal with a low sink density undergoing neutron irradiation at low temperature (T /Tm < 0.2), when sinks contribute to interstitial annihilation, the vacancy and interstitial concentrations as a function of time can be written Eq. (5.11) as: Cv = (K0 KisCst/Kiv )1/2 Ci = (K0 /Kiv KisCst)1/2 (Hint: consider this case to be intermediary to the quasi-steady state and steady state cases such that dCi / dt < 0 and dCv / dt > 0 and write the point defect balance equations as inequalities.) 5.16 Two bi-layer samples with a low sink strength are being irradiated at low temperature as part of a radiation-enhanced diffusion experiment. If the displacement rate of the second sample is five times that of the first sample, what is the difference in the radiation-enhanced diffusion coefficient?

References

227

References 1. Rothman SJ (1983) Effects of irradiation and diffusion in metals and alloys. In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, pp 189–211 2. Sizemann R (1978) J Nucl Mater 69/70:386–412 3. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Service, Springfield, VA 4. Lam NQ (1975) J Nucl Mater 56:125–135 5. Wiedersich H (1986) In: Johnson RA, Orlov AN (eds) Physics of Radiation Effects in Crystals. Elsevier Science, New York, p 237 6. Matteson S, Roth J, Nicolet M (1979) Rad Eff 42:217–226 7. Heald PT, Harbottle JE (1977) J Nucl Mater 67:229–233 8. Brailsford AD, Bullough R (1972) J Nucl Mater 44:121–135

Part II

Physical Effects of Radiation Damage

6 Radiation-Induced Segregation

A profound consequence of irradiation at elevated temperature is the spatial redistribution of solute and impurity elements in the metal. This phenomenon leads to enrichment or depletion of alloying elements in regions near surfaces, dislocations, voids, grain boundaries, and phase boundaries. Figure 6.1 shows a plot of solute element profiles across a grain boundary in stainless steel irradiated in a reactor to a dose of several dpa at about 300 ◦C. Note that there is significant depletion of chromium, molybdenum and iron and enrichment of nickel and silicon. Such drastic changes at the grain boundary will cause changes in the local properties of the solid and may induce susceptibility to a host of processes that can degrade the integrity of the component. For this reason, understanding radiation-induced segregation (RIS) is of great importance for reactor performance.

Fig. 6.1. Radiation-induced segregation of Cr, Ni, Si and P at the grain boundary of a 300 series stainless steel irradiated in a light water reactor core to several dpa at ∼ 300 ◦C (after [1])

232

6 Radiation-Induced Segregation

First postulated by Anthony in 1972 [2], and observed by Okamoto and Weidersich in 1973 [3], RIS has its origin in the coupling between defect fluxes and fluxes of alloying elements. Irradiation produces point defects and defect clusters with an approximately random distribution throughout the material. Those defects that are mobile and escape recombination are re-incorporated into the crystal structure at dislocations, grain boundaries and other defect sinks. As shown in Chap. 5, point defects flow to spatially discrete sinks. Since the motion of atoms causes the motion of defects, atom fluxes are associated with defect fluxes. Any preferential association of defects with a particular alloying component and/or preferential participation of a component in defect diffusion will couple a net flux of the alloying element to the defect fluxes. The flux of an element causes its buildup or depletion in the vicinity of defect sinks and, therefore, concentration gradients in initially homogeneous alloy phases. The concentration gradients induce back diffusion of the segregating elements, and a quasi-steady state may be set up during irradiation whenever the defect-driven alloying element fluxes are balanced by diffusion-driven back diffusion.

Fig. 6.2. Schematic of radiation-induced segregation in a binary, 50% A–50% B system showing (a) the development of the vacancy concentration profile by the flow of vacancies to the grain boundary balanced by an equal and opposite flow of A and B atoms, but not necessarily in equal numbers, (b) the development of the interstitial concentration profile by the flow of interstitials to the grain boundary balanced by an equal and flow of A and B atoms migrating as interstitials, but not necessarily in equal numbers, (c) the resulting concentration profiles for A and B

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

233

Figure 6.2 presents a schematic of processes driving segregation in a binary, 50%A–50%B alloy, under irradiation at an elevated temperature. As described in Chap. 5, vacancies and interstitials flow to the grain boundary causing a concentration profile to develop. In the case of vacancies (Fig. 6.2a) the flux of vacancies to the grain boundary is balanced by an equal flux of atoms in the opposite direction. However, if the participation of A atoms in the vacancy flux is larger than the atom fraction in the alloy (and consequently the participation of B atoms is less), then there will be a net loss of A atoms, and a net gain of B atoms at the boundary, giving rise to concentration gradients, such as shown in Fig. 6.2c. Considering interstitials, their flux to the grain boundary is also made up of a flux of A and B atoms. If the participation of B atoms in the interstitial flux is greater than the atom fraction in the alloy (and necessarily, the participation of A atoms in the flux is less than the atom fraction in the alloy) then a net increase in B atoms and a corresponding net decrease in A atoms will result. These processes are shown in Fig. 6.2b. This example shows that both vacancy and interstitial flow to the grain boundary can result in the net accumulation of one alloying element and a corresponding depletion of the other alloying element. Whether element A enriches or depletes when both processes are included depends on the relative strengths of atom association with the respective defect fluxes. In this chapter, we will focus on radiation-induced segregation in concentrated binary and ternary alloy systems and we will explore the dependence of RIS on temperature, dose and dose rate.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys To distinguish a concentrated alloy from a dilute alloy, it will be assumed that a concentrated alloy is one in which the substitutional solute concentration is above a few percent. The following segregation model is also well-suited to describe alloy systems with significant atomic size differences, including the limit in which the undersized component is present in dilute solution. The model for solute segregation as developed by Wiedersich [4] follows. We will consider a binary solid solution of elements A and B which are distributed randomly throughout the solid. Due to irradiation the local vacancy and interstitial concentrations change with time according to the point defect balance equations:

∂ Cv = −∇Jv + K0 − R ∂t ∂ Ci = −∇Ji + K0 − R , ∂t

(6.1)

where −∇Jv and −∇Ji are the divergences of the vacancy and interstitial fluxes, respectively, K0 is the Frenkel pair production rate and R = KivCiCv , is the rate of

234

6 Radiation-Induced Segregation

recombination of vacancies and interstitials. Note also that we have dropped the vector notation for sake of simplicity and thus, we will need to keep track of direction. Equations (6.1) are identical to Eq. (5.1) in the absence of sinks and with the gradient term included. The conservation equations for the alloying elements A and B are:

∂ CA = −∇JA ∂t ∂ CB = −∇JB . ∂t

(6.2)

The defect and atom fluxes in Eqs. (6.1) and (6.2) arise from forces due to chemical potential gradients. In reality, the equations should be solved for chemical potential, but for simplicity, we will use relations between fluxes and concentration gradients. The coupling between atom and defect fluxes is based on simple physical models. Note that in the case of self-ion bombardment, we would also include a production term due to the implanted element concentration. It is assumed that diffusive motions of A and B atoms occur only by vacancy and by interstitial jumps. An important coupling between atom and defect fluxes is that a flux of interstitials drives a flux of A and B atoms, equal in size and direction to that of the interstitials, across any fixed lattice or “marker” plane: Ji = JAi + JBi ,

(6.3)

and, similarly, a flux of vacancies drives a flux of A and B atoms equal in size, but opposite in direction, across the marker plane: Jv = − (JAv + JBv ) .

(6.4)

In Eqs. (6.3) and (6.4) and in subsequent notation, the subscripts indicate the species of flux considered, and superscripts the complementary species by which the flux occurs. In general, the division of vacancy and interstitial fluxes via A and B atoms will not be in the same proportion as the atom fractions in the alloy, NA , NB . That is, vacancies may migrate preferentially via B atoms and interstitials via A atoms, as described earlier and shown in Fig. 6.2. The fluxes of atoms and defects can be expressed in terms of the gradients of the different species by the partial diffusion coefficient: 1 DvA = λv2 zv Nv ωAv fAv , 6

(6.5)

where ωAv is the jump frequency with which an A atom exchanges with a vacancy on a given neighboring site, Nv is the atomic fraction of vacancies, zv is the number of nearest neighbors to the A atom, and λv is the jump distance. The term fAv is the correlation factor for A atoms migrating by vacancies, which accounts for the greater than random probability that after an initial jump, subsequent jumps of the A atom will have a displacement component opposite to that of the initial jump.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

235

In alloys, f is highly composition-dependent and is neglected in the following for simplicity, giving: 1 DvA = λv2 zv Nv ωAv , 6

(6.6)

and the partial diffusion coefficient for vacancies via A atoms is: 1 2 A DA v = λv zv Nv ωv . 6

(6.7)

Note than ωAv = ωvA (= ωAv ) since either jump frequency involves the exchange of a given A atom–vacancy pair. Combining those factors on the RHS of Eqs. (6.6) and (6.7) that are common to both, the diffusivity coefficient is defined as: 1 dAv = λv2 zv ωAv , 6

(6.8)

so that we have: DvA = dAv Nv DA v = dAv NA .

(6.9)

For B atoms, the complementary equations are; DvB = dBv Nv DBv = dBv NB

(6.10)

with 1 dBv = λv2 zv ωBv , 6

(6.11)

where ωBv is the effective exchange-jump frequency of a B atom–vacancy pair that includes a factor accounting for possible binding or repulsion between vacancies and B atoms. The partial diffusion coefficients of A and B atoms via interstitials, and interstitials via the elements, provided migration occurs by an interstitial mechanism, are similarly: 1 DiA = λi2 zi Ni ωAi , 6

(6.12)

which is analogous to Eq. (6.6) We are, however, neglecting the fact that interstitial migration is more complex because more than one atom is significantly involved in any interstitial jump. The partial diffusion coefficients for interstitials are thus: DiA = dAi Ni DA i = dAi NA

(6.13)

236

6 Radiation-Induced Segregation

and DiB = dBi Ni DBi = dBi NB .

(6.14)

The expression for dAi and dBi will depend on the interstitialcy mechanism and will be more complicated than Eqs. (6.8) and (6.11). In writing the partial diffusion coefficients in the form D = dN, we further assume that the spatial dependence resides in the factor N, whereas the ds are composition-independent. The “average” or “total” diffusion coefficients for the various species are Dv = dAv NA + dBv NB Di = dAi NA + dBi NB

(6.15)

DA = dAv Nv + dAi Ni DB = dBv Nv + dBi Ni .

(6.16)

Using the partial and total diffusion coefficients we can write the fluxes of atoms and defects with respect to a coordinate system fixed on the crystal lattice: JA = −DA χ ∇CA + dAv NA ∇Cv − dAi NA ∇Ci JB = −DB χ ∇CB + dBv NB ∇Cv − dBi NB ∇Ci

(6.17)

Jv = dAv Nv χ ∇CA + dBvNv χ ∇CB − Dv ∇Cv = (dAv − dBv ) Nv χ ∇CA − Dv ∇Cv Ji = −dAi Ni χ ∇CA − dBi Ni χ ∇CB − Di ∇Ci

(6.18)

= − (dAi − dBi ) Ni χ ∇CA − Di ∇Ci ∂ ln γA ∂ ln γB where χ = 1 + = 1+ , accounts for the difference between ∂ ln NA ∂ ln NB the chemical potential gradient (the true driving force for the diffusion of A and B atoms) and the concentration gradient, and γA and γB are activity coefficients. The second equality in the expressions for Jv and Ji is obtained by neglecting small perturbations arising from the presence of defects, so that ∇CB = −∇CA . This equality describes the Kirkendall effect from the vacancy and interstitial mechanisms, respectively. That is, the difference in the A atom and B atom fluxes in opposite directions past a marker plane must be made up by an appropriate defect flux. Of the four flux equations, Eq. (6.17) to Eq. (6.18), only three are independent because atom fluxes and defect fluxes through a marker plane must balance: JA + JB = −Jv + Ji .

(6.19)

To obtain the atom and defect distributions in time and space, the set of coupled partial differential equations in Eq. (6.1) must be solved for the appropriate initial and boundary conditions. Inserting the fluxes given in Eq. (6.17) to Eq. (6.19) into

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

237

Eq. (6.1) gives:

∂ Cv = ∇ [− (dAv − dBv ) χΩ Cv ∇CA + Dv ∇Cv ] + K0 − R ∂t ∂ Ci = ∇ [(dAi − dBi) χΩ Ci ∇CA + Di ∇Ci ] + K0 − R ∂t ∂ CA = ∇ [DA χ ∇CA + Ω CA (dAi ∇Ci − dAv ∇Cv )] . ∂t

(6.20)

Note that the terms in brackets are just the fluxes, J, of the respective species. The atomic fractions, N have been corrected to volume concentration according to N = Ω C, where Ω is the average atomic volume of the alloy. The equation for element B is CB = 1 − CA when small defect concentrations are neglected. Assuming that steady state has been reached, we can make some qualitative conclusions about the flux equations in Eq. (6.17) to Eq. (6.19). As steady state: JA = JB = 0 ,

(6.21)

and neglecting defect bias effects in the solid: Ji = Jv ,

(6.22)

since vacancies and interstitials are produced and recombine in equal numbers. Eliminating ∇Ci in the relation for JA in Eq. (6.17) using Eqs. (6.19), (6.21) and (6.22) gives: dAv dAi NA NB dBi dAi ∇CA = − (6.23) ∇Cv . χ (dBi NB DA + dAi NA DB ) dBv dBi Equation (6.23) is a relation between the vacancy concentration gradient and the A atom concentration gradient. It is evident that the relation between the direction of the gradient of alloy component A and that of the vacancy gradient is determined dAi dAv and . Recall from Eqs. (6.8) and by the relative magnitude of the ratios dBv dBi (6.11) that: 1 dAv = λv2 zv ωAv 6 1 2 dBv = λv zv ωBv , 6 and

Av ΔSm ωAv = ν exp k

Av −Em exp kT

,

Bv ΔSm ωBv = ν exp k

Bv −Em exp kT

,

therefore:

Bv Av Em − Em dAv , ≈ exp dBv kT

(6.24)

238

6 Radiation-Induced Segregation

since differences in ΔSm between A and B atoms are small. Similarly: Bi Ai Em − Em dAi ≈ exp . dBi kT

(6.25)

During irradiation, the vacancy concentration always decreases towards a defect dAi > sink, and Eq. (6.23) predicts that the element A becomes enriched at sinks if dBi dAv , i.e., if preferential transport of A atoms via interstitials outweighs preferential dBv transport via vacancies and vice versa. Example 6.1. Segregation in a B–25%A alloy Let us look at a B–25%A alloy (where B = Ni and A = Cu), and assume that there is no preferential association of defects with either A or B atoms. Given the following values for migration energies of the two components via vacancies and interstitials: Av ∼ 0.77 eV Em

Ai Em ∼ 0.10 eV

Bv Em ∼ 1.28 eV

Bv Em ∼ 0.15 eV ,

Then, from Eqs. (6.24) and (6.25) we have: dAv dAi 1.28 − 0.77 0.15 − 0.1 − = exp − exp dBv dBi kT kT 0.51 0.05 = exp − exp kT kT

0

Av − ddAi is positive and the concentration gradient of A follows that Since ddBv Bi of vacancies, we have depletion of A at the sink. If this sink is a free surface, then A is depleted at the surface. If it is a grain boundary, then A is depleted at the grain boundary. More A atoms move away from the sink via vacancies than to the sink via interstitials. Figure 6.3 shows the behavior of the A concentration at a temperature of 500 ◦C and a dose rate of 10−3 dpa/s. Note that the drop in the concentration of A at the sink surface is balanced by a buildup behind the depleted zone. With increasing dose the depleted zone increases in depth and width until back diffusion due to the large concentration gradient causes a leveling off and the establishment of a “steady state” condition at t > 104 s.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

239

Fig. 6.3. Concentration profiles of element A in a B–25%A alloy as a function of irradiation Av = 0.77 eV, time at a temperature of 500 ◦C and for a displacement rate of 10−3 dpa/s; Em Bv Ai Bi Em = 1.28 eV, Em = 0.10 eV, Em = 0.15 eV (after [4])

6.1.1 Solution to the Coupled Partial Differential Equations Solution to the system of partial differential equations given in Eq. (6.20) must be obtained numerically. Solutions can be obtained in either planar geometry (free surface) or spherical geometry (grain boundary). In the Perks code [5], segregation of the alloying elements is modeled adjacent to a plane, which is a perfect sink for point defects, such as a grain boundary or a free surface. Another plane is sufficiently far away to model the conditions in the middle of the grain where there are no concentration gradients. The model calculates the concentrations of the major elements by considering the fluxes of each species caused by the migration of point defects created thermally and by irradiation. Point defect losses occur due to mutual recombination and annihilation at fixed sinks, the boundary surfaces and a uniform and time-independent distribution of dislocations. The detailed radiation-induced microstructure is not considered explicitly, but the sink strength can be adjusted with dose to simulate the buildup of sinks in the microstructure. Once the fluxes are calculated, the divergences can be used to perform the time integration required by the continuity equations in Eq. (6.20). The program calculates the concentration of each species independently. An advantage of this method is that any errors in the calculations are evident when the partial concentrations are summed. The deep boundary condition is representative of the bulk material where there are no concentration gradients for atomic and defect species so that the next flux of each species is always zero. The surface or grain boundary is created as a perfect sink for point defects, thus their concentration at the sink is maintained at their initial values ( dCk / dt = 0). In order to conserve atoms in the solid, the atomic fluxes at the boundary are all zero.

240

6 Radiation-Induced Segregation

6.1.2 Interstitial Binding Undersize solutes can tightly bind to interstitials forming interstitial-solute complexes that migrate as solute interstitials. The RIS model described in Sect. 6.1 can account for solute-interstitial binding by accounting for the non-random occupation of interstitials by A and B atoms in the diffusivity coefficients, dAi and dBi , respectively [4]. The concentrations of A and B interstitials are given as: CA exp(EbAi /kT ) , CA exp(EbAi /kT ) + CB CB , CBi = Ci CA exp(EbAi /kT ) + CB

CAi = Ci

(6.26) (6.27)

where EbAi is the average energy gained by converting a B interstitial into an A interstitial. The term EbAi is referred to as the effective A interstitial binding energy. Clearly, solutes that bind to interstitials will undergo enrichment at sinks by virtue of the flow of interstitials to the sink. Example 6.2. Segregation with interstitial binding in Ni–Si Segregation will occur in systems where strong binding of the interstitials to undersize atoms occurs. Consider the system of B–5%A where B is Ni and A is Si and preferential interstitial association with A atoms occurs. Figure 6.4 shows the calculated concentration profile of alloy component A (Si) for an irradiation temperature of 500 ◦C. Note that element A strongly segregates to the surface. This can be understood by referring to the parameters of Eq. (6.27). Av = E Bv = 1.28 eV and E Ai = 0.9 eV, E Bi = 0.15 eV and We have chosen Em m m m a binding energy of EbAi = 1.0 eV so that:

dAv dAi Ai Bi /kT < 0 − = 1 − exp EbAi − Emi + Em dBv dBi and from Eq. (6.23) the surface becomes strongly enriched in Si. The binding energy in part results from the size difference between Ni and Si. Here the solute atom, Si is considerably smaller and is expected to segregate to the surface according to the argument given in Sect. 6.1.3. Results are supported by the preceding calculation and confirmed by experiment. Figure 6.5 shows that segregation of silicon to the surface does indeed occur in a Ni–1%Si alloy irradiated at moderate temperature. It should also be noted that in the Ni– Si system, the solubility limit for Si is ∼ 10 at%, and that segregation of Si to values of above the solubility limit will result in precipitation of Ni3 Si. Hence one important result of irradiation-induced segregation is that it can lead to local solute concentration that exceeds the solubility limit and results in precipitation. Irradiation can also act to stabilize a second phase that would otherwise not be present in thermodynamic equilibrium and vice versa. These processes are discussed in Chap. 9.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

241

Fig. 6.4. Concentration profiles of element A in a B–5%A alloy as a function of irradiaAv = E Bv = tion time at temperature of 500 ◦C and for a displacement rate of 10−3 dpa/s; Em m Ai = 0.90 eV, E Bi = 0.15 eV (after [4]) 1.28 eV, EbAi = 1.0 eV, Em m

Fig. 6.5. Measured concentration vs. depth profiles for a Ni–1%Si alloy irradiated to doses between 3.9 and 8.5 dpa at temperatures between 560 and 660 ◦C with 3.5 MeV 58 Ni+ ions at a displacement rate of ∼ 10−3 dpa/s at the sample surface (after [6])

6.1.3 Solute Size Effect Size difference between solute atoms plays a major role in determining the magnitude and direction of segregation [6]. To reduce the strain energy stored in the lat-

242

6 Radiation-Induced Segregation

tice, undersize solute substitutional atoms will preferentially exchange with solvent atoms in interstitial positions, whereas oversize solute atoms will tend to remain on, or return to, substitutional sites. Strain-energy considerations also predict that vacancies will preferentially exchange with oversize solute atoms. During irradiation at elevated temperatures, the fraction of undersize solute atoms migrating as interstitials, or of oversize solute atoms migrating against the vacancy flux, may therefore greatly exceed the fraction of solute in the alloy. In other words, any variation in size between solute and solvent atoms will cause the chemical composition of the irradiation-induced interstitial and vacancy fluxes toward sinks to differ from the chemical composition of the alloy. This disproportionate participation of misfitting solute atoms in the defect fluxes to sinks will cause a redistribution of solute, which will produce an enrichment of undersize solute and a depletion of oversize solute near defect sinks. Since the surface of an irradiated solid serves as an unsaturable sink for both vacancy and interstitial-type defects, concentration gradients will be created near the surface of alloys that contain misfitting solute atoms during irradiation at appropriate temperatures. Table 6.1 shows the volume misfit for several solute–solvent combinations and the predicted and observed direction of segregation under irradiation. Note that positive misfits should result in depletion (−) at sinks while negative misfits should result in enrichment (+) at sinks. Example 6.3. Segregation driven by the size effect in Ni–1%Al An example of the size effect is the Ni–Al system. According to Table 6.1, Al−v will be less than E Ni−v Al is an oversized solute in the Ni lattice, and Em m since the oversize Al atoms will preferentially exchange with vacancies. AcdAv dAi cording to Eqs. (6.24) and (6.25), > and depletion at the surface is dBv dBi predicted. In fact, measurement of the segregation of Al in Ni–1%Al irradiated to 10.3 dpa at 510 ◦C and to 10.7 dpa at 620 ◦C shows strong depletion of Al at the surface followed by redistribution behind the surface (Fig. 6.6). The buildup of Al just below the surface results in an Al concentration that exceeds the solubility limit and induces second phase formation as discussed in detail in Chap. 9.

6.1.4 Effect of Temperature The temperature dependence of RIS is shown in Fig. 6.7 for a B–25% A alloy, as determined by solution of Eq. (6.20). Note that with increasing temperatures, the dAi dAv and decreases with profile flattens. This is because the difference between dBv dBi increasing temperature. Figure 6.8 shows that the steady state concentration at the sink surface passes through a minimum as a function of temperature and can be explained as follows. At high temperatures, a large thermal vacancy concentration

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

243

Table 6.1. Effect of solute size on radiation-induced segregation (from [7, 8, 9]) Solute–solvent

Volume misfit (%)

Predicted direction of segregation

Observed direction of segregation

Pd–Cu Pd–Fe Pd–Mo Pd–Ni Pd–W Al–Ge Al–Si Al–Zn Fe–Cr Mg–Cd Ti–Al Ti–V Ni–Al Ni–Au Ni–Be Ni–Cr Ni–Ge Ni–Mn Ni–Mo Ni–Sb Ni–Si Ni–Ti Cu–Ag Cu–Be Cu–Fe Cu–Ni ∗ SS–Ni ∗ SS–Cr ∗ SS–Si ∗ SS–C ∗ SS–Mn ∗ SS–Mo ∗ SS–Cu

−20 −27 −3 −26 −2 −37 −45 −19 +4 −19 −3 −26 +52 +55 −29 +1 −5 +32 +31 +21 −16 +57 +44 −34 −8 −7 −3 +5 −3 +54 +3 +36 +9

+ + + + + + + + − + + + − − + − + − − − + − − + + + + − + − − − −

+ + + + + + + + − + + + − − + − + − − − + − − + + + + − +

∗

− −

SS refers to 316 stainless steel from [8]

leads to a high diffusion rate of alloying elements as well as to a high defect recombination rate; the latter reduces the defect fluxes to sinks, and hence, the amount of solute segregation, while the former increases the back diffusion of segregated alloying elements. At low temperatures, the vacancy mobility is low, the radiation-induced excess vacancy concentration is correspondingly high so that defect recombination becomes dominant, and hence the defect fluxes to sinks decrease and segregation is

244

6 Radiation-Induced Segregation

Fig. 6.6. Measured concentration vs. depth profiles for a Ni–1%Al alloy irradiated to 10.3 dpa at 510 ◦C and to 10.7 dpa at 620 ◦C with 3.5 MeV 58 Ni+ ions at a displacement rate of ∼ 10−3 dpa/s at the sample surface (after [6])

Fig. 6.7. Steady state concentration profiles of element A as a function of temperature for the same alloy and irradiation conditions as shown in Fig. 6.3 (after [4])

reduced. At intermediate temperatures, the thermal vacancy concentration becomes insignificant and the radiation-induced excess vacancy concentration is relatively low. The defect recombination rate is low, and hence defects migrate predominantly to sinks and significant segregation occurs.

6.1 Radiation-Induced Segregation in Concentrated Binary Alloys

245

Fig. 6.8. Temperature dependence of grain boundary segregation of Ni, Cr and Fe in a Ni– 18Cr–9Fe alloy irradiated with 3.4 MeV protons at 400 ◦C to 1 dpa and at a displacement rate of 7 ×10−6 dpa/s (after [10])

6.1.5 Effect of Dose Rate Decreasing the dose rate will shift the temperature dependence of RIS to lower temperatures as shown in Fig. 6.9. The shift of the curve toward lower temperatures for lower displacement rates can be explained as follows. At a given temperature, a lower point defect generation rate K0 means the vacancies and interstitials are added to the lattice more slowly, or more widely spaced in time. However, their thermal mobility is unchanged and with the lower numbers of defects in the lattice, the probability of finding a sink vs. recombination is increased. Thus, at a given temperature, lower displacement rates tend to increase the role of the sink over the

Fig. 6.9. Dose rate dependence of grain boundary chromium depletion calculated using the MIK model for RIS (after [11] and [12])

246

6 Radiation-Induced Segregation

role of recombination, resulting in greater segregation. At high temperatures, a lower displacement rate means that irradiation-produced vacancies will have less of an impact, so that their effect on segregation is less than that at higher dose rate and the amount of segregation drops with decreasing dose rate.

6.2 RIS in Ternary Alloys Engineering alloys are rarely simple binary alloys. Most structural alloys contain many solutes, each with a specific role in the properties of the alloy. Because of the significance of structural stainless steels that are predominantly composed of iron, chromium and nickel, we will reproduce the development of the time and spacedependent concentration equations for a ternary alloy under irradiation. The following description is a condensation of that given by Lam et al. [13] for a ternary alloy whose components A, B and C are present in concentrations CA , CB and CC (number of atoms per unit volume). We start by writing the defect fluxes partitioned into those occurring via A, B and C atoms in the alloy according to: Ji = JiA + JiB + JiC Jv = JvA + JvB + JvC ,

(6.28)

where the subscripts indicate the species of flux (interstitial or vacancy) and the superscripts indicate the complementary species by which the flux occurs (atom A, B, or C). The partial interstitial fluxes are in the same direction as the corresponding atom fluxes while the partial vacancy fluxes are in the opposite direction to the atom fluxes: JiA = JAi ; JvA = −JAv ;

JiB = JBi ;

JiC = JCi

JvB = −JBv ;

JvC = −JCv ,

(6.29)

and Eq. (6.25) can be written as: Ji = JAi + JBi + JCi Jv = − (JAv + JBv + JCv ) .

(6.30)

These equations express the coupling between defect and atom fluxes across any fixed lattice plane. As with the defect compositions, the alloy composition in time and space can be described by the conservation equations:

∂ CA = −∇ · JA ∂t ∂ CB = −∇ · JB ∂t ∂ CC = −∇ · JC , ∂t

(6.31)

6.2 RIS in Ternary Alloys

247

where JA , JB and JC are the total fluxes of the alloying elements, which can be partitioned into partial fluxes occurring by vacancies and interstitials: JA = JAv + JAi JB = JBv + JBi JC = JCv + JCi

(6.32) .

The defect and atom fluxes are expressed in terms of the concentration gradients of the different species: Jki (≡ Jik ) = −Dik χ ∇Ck − Dki ∇Ci Jkv (≡ −Jvk ) = −Dvk χ ∇Ck + Dkv ∇Cv ,

(6.33)

where k = A, B or C, χ is the thermodynamic factor which relates the concentration gradient to the chemical potential gradient of atoms (as in Eqs. (6.17) and (6.18)), and Dik Dvk , Dki and Dkv are the partial diffusion coefficients of atoms k by interstitials, and vacancies, and of interstitials and vacancies by atoms, respectively. The partial diffusion coefficients have the form: Dkj = dk j N j Dkj = dk j Nk ,

(6.34)

where j = i or v, N j = Ω C j and Nk = Ω Ck are the atomic fractions of defects and of k atoms, respectively, Ω is the average atomic volume in the alloy, and dk j are the diffusivity coefficients for conjugate atom-defect pairs k j: 1 dk j = λk2 zk ωkeffj . 6

(6.35)

Here λk is the jump distance, zk the coordination number, and ωkeffj the effective jump or exchange frequency of the pair. The total diffusion coefficients for interstitials and vacancies are defined as: Di = ∑ dki Nk k

Dv = ∑ dkv Nk ,

(6.36)

k

and for atoms: Dk = dki Ni + dkvNv .

(6.37)

For alloy systems in which atoms of one alloy component interact with interstitials to form bound atom–interstitial complexes, the non-random occupation of interstitials by A, B, and C atoms is accounted for in the same manner as for a binary alloy system. For preferential A atom–interstitial binding, we have by analogy with Eqs. (6.26) and (6.27):

248

6 Radiation-Induced Segregation

CA exp(EbAi /kT ) , CA exp(EbAi /kT ) + CB + CC CB CBi = Ci , Ai CA exp(Eb /kT ) + CB + CC CC CCi = Ci , Ai CA exp(Eb /kT ) + CB + CC

CAi = Ci

(6.38)

where EbAi is the average energy gained by converting a B interstitial or a C interstitial into an A interstitial. From Eqs. (6.31), (6.33), (6.34), (6.35) and (6.28), the defect and atom fluxes with respect to a coordinate system fixed on the crystal lattice are: Ji = −(dAi − dCi )Ω Ci χ ∇CA − (dBi − dCi )Ω Ci χ ∇CB − Di ∇Ci Jv = (dAv − dCv)Ω Cv χ ∇CA + (dBv − dCv)Ω Cv χ ∇CB − Dv ∇Cv JA = −DA χ ∇CA + dAv Ω CA ∇Cv − dVi Ω CA ∇Ci JB = −DB χ ∇CB + dBvΩ CB ∇Cv − dVi Ω CB ∇Ci

(6.39)

JC = −DC χ ∇CC + dVv Ω CC ∇Cv − dCi Ω CC ∇Ci . Small perturbations arising from the presence of point defects are neglected so that CA +CB +CC = 1 and ∇CC = −(∇CA + ∇CB ). Of the five fluxes in Eq. (6.39), only four are independent because the defect and atom fluxes across a marker plane must balance: JA + JB + JC = Ji − Jv .

(6.40)

A system of four coupled partial differential equations describing the space and time dependence of the atoms and defects in the solid is determined by substituting the defect and atom fluxes given by Eq. (6.39) into Eqs. (6.31) and (6.1):

∂ Cv ∂t ∂ Ci ∂t ∂ CA ∂t ∂ CB ∂t

= ∇ · [−(dAv − dCv)Ω Cv χ ∇CA −(dBv −dCv )Ω Cv χ ∇CB + Dv ∇Cv ] + K−R = ∇ · [(dAi − dCi )Ω Ci χ ∇CA + (dBi − dCi )Ω Ci χ ∇CB + Di ∇Ci ] + K − R = ∇ · [DA χ ∇CA + Ω CA (dAi ∇Ci − dAv ∇Cv )] = ∇ · [DB χ ∇CB + Ω CB (dBi ∇Ci − dBv∇Cv )] .

(6.41)

Numerical solutions of Eq. (6.41) are obtained for a planar sample under irradiation. The grain boundary is equated to a free surface and the calculations are performed for only a single grain, taking advantage of the symmetry of the problem. The initial conditions are those for thermodynamic equilibrium of the alloy. Conditions at the boundary are defined as follows. At the grain center, all

6.2 RIS in Ternary Alloys

249

concentration gradients are set equal to zero. At the grain boundary, the concentrations of interstitials and vacancies are fixed at their thermal equilibrium values. The grain boundary atom concentrations are determined by the conservation of the numbers of atoms in the specimen. Atom concentrations are assumed to be initially uniform. Parameters used in the calculation of segregation in Fe–Cr–Ni alloys are given in [13] for the Lam model and in [5] for the Perks model. Equations (6.41) can be solved at steady state to provide a relationship between the vacancy gradient and the atom gradient. This relationship is known as a determinant, M and is a function of the concentrations and diffusivities. The determinant for a three-component alloy is determined in the same way as was done for the binary alloy case Eq. (6.23) and is given by [14]:

Mj =

∇C j = ∇Cv

d jvC j Dj

dkiCk d jiC j − Dj k = j Dk

∑

χ∑ k

dkvCk k = j Dk

∑

dkiCk Dk

.

(6.42)

The determinant can be used to help determine the primary mechanism of segregation in Fe–Cr–Ni alloys. Table 6.2 shows the determinant calculated for Cr, Fe, and Ni for a total of seven alloys assuming that preferential coupling with the vacancy flux causes the segregation, i.e., setting the interstitial diffusion coefficients for Cr, Fe, and Ni to be equal to each other. The segregation trends (enrichment or depletion at the grain boundary) for Cr, Fe, and Ni that were measured on the grain boundaries of these alloys by Auger electron spectroscopy (AES) and energy dispersive spectroscopy in scanning transmission electron microscopy (STEM/EDS) are also listed. For each alloy where the determinant for the element is positive, depletion occurs; where the determinant is negative enrichment occurs. Note that for each element in each of the seven alloys studied, the sign of the determinant agrees with the measurement (by either STEM/EDS or AES) and calculation. This example also shows that while chromium always depletes and nickel always enriches, iron can either enrich or deplete depending on the relative concentrations of nickel and chromium. Table 6.2. Segregation behavior in Ni–Cr–Fe and Fe–Cr–Ni alloys compared to inverse Kirkendall predictions. Determinants (M) calculated using Eq. (6.42) Alloy

MCr MFe

MNi

Ref. Cr

Fe

Ni

Analysis method

Ni–18Cr Ni–18Cr–9Fe Fe–16Cr–24Ni Fe–20Cr–24Ni Fe–24Cr–24Ni Fe–24Cr–19Ni Fe–20Cr–9Ni

3.9 5.0 4.0 5.0 6.3 6.5 5.0

−3.9 −5.4 −7.6 −7.4 −8.5 −4.7 −2.0

[14] [15] [16] [16] [16] [16] [16]

— Depletes Depletes Depletes Depletes Enriches Enriches

Enriches Enriches Enriches Enriches Enriches Enriches Enriches

AES&STEM/EDS AES&STEM/EDS AES AES&STEM/EDS AES AES AES&STEM/EDS

— 0.4 3.6 2.4 1.8 −1.8 −3.0

Depletes Depletes Depletes Depletes Depletes Depletes Depletes

250

6 Radiation-Induced Segregation

In the Fe–Cr–Ni system, Cr is the fast diffuser and Ni is the slow diffuser and Fe is between the two. When the nickel level is high relative to the Cr level, the large amount of enrichment of Ni at the grain boundary cannot be fully compensated by depletion of Cr, so Fe also must deplete. But when the Cr level is high relative to Ni the reverse occurs and Fe enriches. Note that Cr and Ni do not exactly cancel as can be seen in the case of the Fe–24Cr–24Ni alloy in which Ni enrichment is stronger than Cr depletion and Fe must also deplete. This example exposes a key process in RIS, the role of composition in the segregation behavior. When the composition near a sink starts to change, the diffusivities of the elements in that region will change also as diffusion is compositiondependent. The effect of changing local composition needs to be accounted for in order to properly determine the extent of RIS, as will be covered in the next section.

6.3 Effect of Local Composition Changes on RIS We have established that RIS occurs because of differences in the coupling of the various solutes with defects. Further, the difference in the strength of the coupling influences the degree of segregation. Therefore, when the concentration near the sink is significantly different from that in the bulk, the diffusivities of the solutes will change as well, and this change needs to be accounted for in order to accurately determine the composition profile [12]. The Perks model can be modified to include both composition-dependent diffusivities. In the Perks model, the rate of segregation of element k by defect j is described by a diffusivity of the general form given by Eq. (6.24): j kj −Em Sm 2 exp , dkj = 1/6λj zj ν exp k kT or in simplified notation: kj −Em kj dkj = d0 exp , kT

(6.43) kj

where the pre-exponential terms are lumped into a single term, d0 . In most solutions to Eq. (6.41), the migration energies for each element are assumed to be equal, with differences in segregation rates arising from differences in the pre-exponential factors. To account for diffusion in a solution of varying composition, the migration energy term in the exponential must be described as a function of composition [11, 15, 16] as presented in the following paragraphs. For an atom to migrate (Cr migrating in a Fe–Cr–Ni lattice will be used as an example), it must move fromits equilibrium position in the lattice (with equilibrium kj −Em kj ) and travel through a position of maximum potential energy dkj = d0 exp kT

6.3 Effect of Local Composition Changes on RIS

251

Fig. 6.10. Determination of the migration energy for an atom–vacancy exchange in an Fe– Cr–Ni alloy (after [12])

kj −Em (known as the saddle point, with saddle point energy dkj = ), bekT fore moving to a new lattice site. This relationship between the energies is shown schematically in Fig. 6.10. For atom – vacancy exchnge the migration energy is the difference between the saddle point energy and the equilibrium energy: kj d0 exp

Cr-v Cr Cr = ESFe-Cr-Ni − Eeq . Em

(6.44)

In a simple model, the equilibrium energy can be described as the interaction energy between nearest neighbors: Cr-v Eeq = Z [CCr ECrCr + CNi ENiCr + CFe EFeCr + Cv ECr-v ] ,

(6.45)

where Z is the number of nearest neighbors, C is the atomic concentration of atoms and/or defects, and Ekj is the pair interaction energy between an atom k and an atom or vacancy j. Pair interaction energies between unlike neighbors are defined to be a linear average of the like atom pair energies minus any ordering energy: ENiCr =

ENiNi + ECrCr ord − ENiCr . 2

(6.46)

Combining Eq. (6.44) to Eq. (6.46) and requiring that CFe + CCr + CNi = 1, the migration energy for Cr, Ni and Fe via vacancies can be expressed as:

1 CNi CFe Cr-v Em (C E E = ESCr − Z + 1) E + + + C E FeFe v Cr CrCr NiNi Cr-v Fe–Cr–Ni 2 2 2 ord ord + ZCNi ENiCr + ZCFe EFeCr (6.47a)

1 CCr CFe Ni-v Em (C E E = ESNi − Z + 1) E + + + C E FeFe v Ni-v Ni NiNi CrCr Fe-Cr-Ni 2 2 2 ord ord + ZCFe EFeNi + ZCCr ENiCr

(6.47b)

252

6 Radiation-Induced Segregation

Fe-v Em = ESFe Fe-Cr-Ni − Z

1 CCr CFe (CFe + 1) EFeFe + ECrCr + ENiNiFe-v + Cv ENi-v 2 2 2

ord ord + ZCFe EFeCr + ZCNi EFeNi

(6.47c)

In order to determine the migration energies in Eq. (6.47), pair interaction energies and saddle point energies must be calculated. For like atoms, the pair interaction energy is the cohesive energy, Ecoh divided by the number of nearest neighbor bond pairs: Cr ECrCr = Ecoh /(Z/2) ,

(6.48a)

Fe EFeFe = Ecoh /(Z/2) , Ni ENiNi = Ecoh /(Z/2) .

(6.48b) (6.48c)

Since pure Fe and pure Cr occur in the bcc structure, the energy required to convert Fe and Cr to the fcc structure for application to stainless steels must be included in the determination of ECrCr and EFeFe to properly describe the equilibrium energy: f cc f cc bcc ECrCr = ECrCr + ΔGbcc→ , Cr

(6.49a)

f cc EFeFe

(6.49b)

f cc bcc = EFeFe + ΔGbcc→ Fe

.

Pair interaction energies between unlike atoms are determined from the average value of the like-atom pair energies less any ordering energy: (ENiNi + ECrCr ) ord − ENiCr , 2 (EFeFe + ECrCr ) ord − EFeCr EFeCr = , 2 (EFeFe + ENiNi ) ord − EFeNi EFeNi = . 2 ENiCr =

(6.50a) (6.50b) (6.50c)

Finally, the pair interaction energy for atoms and vacancies is fitted to the formation energy of the pure metal and is given by: Cr Ecoh + EfCr-v ECr-v = , (6.51a) Z Ni Ecoh + EfNi-v ENi-v = , (6.51b) Z Fe Ecoh + EfFe-v EFe-v = , (6.51c) Z where Efk-v is the vacancy formation energy in pure k. The last quantity remaining to be determined is the saddle point energy, which is calculated using the saddle point energy of pure Fe, Cr, and Ni. The saddle point

6.4 Effect of Solutes on RIS

253

energy in the pure metal is calculated to reproduce the vacancy migration energy in the pure metal. For example, assuming that in pure Cr both an atom and a vacancy are extracted and placed at a saddle point, then the energy to extract the Cr atom is given by: ECr = Z(CCr ECrCr + Cv ECr-v ) .

(6.52)

The energy to extract the vacancy is: Ev = Z(Cv Evv + CCr ECr-v )

(6.53)

Since CCr +Cv = 1 in a pure metal and since Cv CCr , the sum of ECr +Ev becomes: ECr + Ev = Z(ECrCr + ECr-v ) .

(6.54)

Equation (6.54) represents the equilibrium energy for pure Cr. We want to place the atom at a saddle point with an energy such that: Cr-v Cr Cr = ESpure − (ECr + Ev) = ESpure − Z(ECrCr + ECr-v ) . Em

(6.55)

The saddle point energy in the pure metal is then given as: Cr Cr-v ESpure = Em + Z(ECrCr + ECr-v ) .

(6.56)

This approach, described in the modified inverse Kirkendall (Perks) model called the MIK model [12], was used to model RIS and results were compared to measurements taken on a range of Fe-base and Ni-base austenitic alloys irradiated at temperatures from 200 to 600 ◦C and at doses up to 3 dpa. The RIS results shown in Fig. 6.11 clearly demonstrate the importance of accounting for composition changes near the sinks in the determination of the RIS composition profiles. The MIK model calculations agree with AES measurements of grain boundary nickel concentration in irradiated Fe–20Cr–24Ni much better than the original Perks model. Also, over a range of alloys, doses and irradiation temperatures (Fig. 6.12) the inclusion of local composition changes on RIS results in much better agreement with the data. These data also serve to illustrate the importance of vacancies in RIS in Fe–Cr–Ni alloys at intermediate temperatures. The MIK model calculations did not include either interstitial binding (that is, Ebik = 0) or preferential participation of any of the alloying elements in the interstitial flux. Excellent agreement between model and measurement is achieved solely by preferential participation of alloying elements in the vacancy flux. Hence, in the Fe–Cr–Ni system, atom migration via vacancies appears to be the dominant mechanism of RIS.

6.4 Effect of Solutes on RIS The presence of impurities in a solid can influence the propensity for RIS at the grain boundary. It has been hypothesized that solutes that are oversized or undersized with

254

6 Radiation-Induced Segregation

Fig. 6.11. The modified inverse Kirkendall (MIK) model result compared to the Perks model result and to measurement showing the importance in accounting for the changing local composition at sinks in RIS. Experiment was conducted on Fe–20Cr–24Ni using 3.2 MeV protons at 400 ◦C and at a displacement rate of 7 ×10−6 dpa/s (after [12])

Fig. 6.12. MIK model applied to several alloys under a range of doses and temperatures and comparison to measurement (after [2])

6.4 Effect of Solutes on RIS

255

respect to the lattice atoms can act as traps for vacancies or interstitials. Trapping of point defects by solutes could increase the fraction of vacancies and interstitials undergoing mutual recombination, thus reducing the fraction flowing to sinks, and hence, the degree of segregation. Mansur and Yoo [17] generalized the point defect balance equations to include point defect trapping. Trapping is accommodated by subtracting and adding terms corresponding to trapping and recombination at traps, and the release of point defects from traps. In addition, equations describing the conservation of the trapped defects are also added. As a result, the point defect balances, from Eq. (6.1), are given as follows: Free vacancies:

∂ Cv = ∇ · Dv ∇Cv + K0 − KivCiCv ∂t + ∑ τvl−1Cvl − Cv ∑ Kil Cil − Cv ∑ κvl (Clt − Cvl − Cil ) − KvCv . l

l

(6.57)

l

Free interstitials:

∂ Ci = ∇ · Di ∇Ci + K0 − KivCiCv ∂t + ∑ τil−1Cil − Ci ∑ Kvl Cvl − Ci ∑ κil (Clt − Cvl − Cil ) − KiCi . l

l

(6.58)

l

In Eqs. (6.57) and (6.58), the summations extend over the l = 1, 2, . . ., n types of traps. Similarly, the following equations apply to each of the l = 1, 2, . . ., n types of traps. Traps (concentration in general is a function of position and time):

∂ Clt = fl (r,t) . ∂t

(6.59)

Trapped vacancies: t ∂ Cvl = Cv κvl (Clt − Cvl − Cil ) − τvl−1Cvl − Ci Kvl Cvl . ∂t

(6.60)

Trapped interstitials:

∂ Cilt = Ci κil (Clt − Cvl − Cil ) − τil−1Cil − Cv Kil Cil . ∂t

(6.61)

In Eqs. (6.57) and (6.58), the first three terms are the same as in Eq. (6.1). The remaining terms have the following meaning. Referring to the equation for free vacancies, the fourth term is the release of trapped vacancies from the sink and the variable τvl−1 is the mean time that the vacancy is trapped at the lth trapping site. The mean trapping time is denoted by τ jl = (b2 /D0j ) exp[(Ebjl + Emj )/kT ], where j denotes i j

or v, D0j is the pre-exponential of the diffusion coefficient [D j = D0j exp(−Em /kT )], b is the order of atomic distance, Ebjl is the binding energy of the point defect at

256

6 Radiation-Induced Segregation j

the lth type trap, and Em is the point defect migration energy. The fifth term is the recombination rate of vacancies with trapped interstitials, where Kil is the recombination rate constant for that reaction and is given by Kil = 4π ril Dv or Kvl = 4π rvl Di , where ril and rvl denote the respective radii of the recombination volumes. The sixth term describes the trapping of free vacancies at a trap of type l. The concentration − C ) accounts for the fact that the fraction C /Ct + C /Ct difference (Clt − Cvl il vl il l l traps of type l are already occupied by vacancies and interstitials and hence, are not available as traps for free defects. It also accounts for the fact that a given trap may have a binding energy for both vacancies and interstitials but would not trap both simultaneously, since when one is trapped, the site is then a recombination center. D and κ = 4π r D denote the capture coefficients similar to The terms κvl = 4π rvl v il il i and r are the capture radii of the trap type l recombination coefficients, and the rvl il for the respective point defects. Finally, the seventh term is the loss of defects to all internal sinks and Kv describes the rate constant for all sinks. Equation (6.57) through Eq. (6.61) are substituted for the vacancy and interstitial concentrations in Eq. (6.41) and solved in the same manner as before in a version of the MIK code designated MIK-T. The results of trapping in Fe–16Cr–13Ni containing an oversized solute concentration of 1% is shown in the plot of grain boundary chromium content vs. dose for the case of irradiation at a dose rate of 10−5 dpa/s at a temperature of 400 ◦C and for interstitial and vacancy binding energies up 1.0 eV (Fig. 6.13a). Note that high binding energies on the order 1.0 eV are required for trapping to reduce the amount of RIS. The main effect is a reduction in the amount of grain boundary Cr depletion, but a secondary effect is a slowing of the rate of segregation with dose. Figure 6.13b shows that trapping moves the temperature at which RIS is a maximum to a slightly lower temperature. Figure 6.14 shows the effect of oversize solute addition on grain boundary chromium depletion and nickel enrichment in Fe–Cr–Ni alloys irradiated with protons, and that experimental results qualitatively follow those of the model. As successful as these models are in predicting the direction and magnitude of segregation, they are very incomplete. The models have been developed for binary and ternary systems only, whereas real engineering alloys may contain 10–20 alloying elements. Even though some may be present in very small quantities, they can exert a very large influence on the behavior of the alloy. The Perks and MIK models apply only to solute atoms and not to small interstitial atoms such as B, C and N. Further, many of the thermodynamic parameters required for accurate simulation of RIS are unknown and must be estimated, introducing uncertainty into the results. Despite these shortcomings, they can serve to rationalize to RIS in real systems.

6.5 Examples of RIS in Austenitic Alloys As stated earlier, RIS is an extremely important problem in structural materials exposed to irradiation at elevated temperatures. The changes in grain boundary composition can give rise to microstructure changes (precipitation, dislocation loop structure, void structure) in addition to changes in susceptibility to processes such as

6.5 Examples of RIS in Austenitic Alloys

257

Fig. 6.13. Calculated grain boundary Cr composition (a) as a function of binding energy for the MIK-T model at 400 ◦C and 1 ×10−5 dpa/s for Fe–16Cr–13Ni, and (b) as a function of temperature at a constant dose rate of 10−5 dpa/s at 3 dpa. Percent difference calculated by (MIK-T – MIK)/MIK∗ 100% (after [18])

258

6 Radiation-Induced Segregation

Fig. 6.14. Grain boundary Cr and Ni composition for reference and oversize impurity-doped Fe–Cr–Ni alloys irradiated at 400 ◦C to 3.0 dpa (Zr) and 2.5 dpa (Hf) (after [18] and [19])

intergranular corrosion and stress corrosion cracking. For example, we determined that Cr always depletes in irradiated stainless steels, and the loss of chromium at grain boundaries could cause an increased susceptibility to intergranular corrosion and intergranular stress corrosion cracking, since chromium provides passivity to the alloy by forming a very thin, protective, Cr2 O3 film. As will be discussed in Chap. 15, with increases in dose above some pseudo-threshold level, the amount of intergranular stress corrosion cracking (IGSCC), measured as the percentage of the fracture surface that displays intergranular facets, increases steeply in slow strain rate tests in 288 ◦C normal water chemistry used in boiling water reactors (BWR). Figure 6.15 shows that the grain boundary Cr content also decreases rapidly with dose due to RIS. The loss of Cr may raise the susceptibility of the alloy to IASCC, although other changes are occurring in the microstructure at the same time. Silicon is also observed to segregate very strongly with dose, as shown in Fig. 6.16 for austenitic stainless steels irradiated at ∼ 288 ◦C. These measurements of high levels of Si were made by STEM/EDS. Due to the spatial resolution limit of this technique, the actual grain boundary level of Si may be underestimated by as much as a factor of 3–5, giving concentrations of over 20% Si at the grain boundary. Since Si is soluble in high-temperature water, it is possible that it could be enhancing dissolution at the grain boundary giving rise to increased rates of intergranular corrosion (IGC) and IGSCC.

6.6 RIS in Ferritic Alloys

259

Fig. 6.15. Dependence of grain boundary chromium concentration on dose for a range of 300 series stainless steels irradiated under various conditions. Note that RIS increases with dose through about 5 dpa after which the change is minimal (after [20]) Fig. 6.16. Grain boundary segregation of silicon in 300 series austenitic alloys irradiated with neutrons or protons to 13 dpa

6.6 RIS in Ferritic Alloys RIS is also of significance in ferritic steels, particularly pressure vessel steels where the grain boundary segregation of interstitial impurities such as P can have significant consequences for grain boundary embrittlement. Compared to austenitic steels, little work has been done on the segregation of alloying elements in ferritic alloys. Segregation models for interstitial impurities are not as well-developed as for sub-

260

6 Radiation-Induced Segregation

stitutional solutes. Faulkner [21] has reviewed the segregation data and mechanisms and suggests that RIS in ferritic steels is by defect–impurity complexes and that site competition by other elements at the boundary plays a significant role determining in the amount of segregation of a particular impurity. Focusing on the behavior of P, it is assumed that migration by self-interstitial phosphorus complexes is fast such that the concentration remains uniform across the grain boundary plane. The maximum grain boundary concentration of phosphorus is given by: ⎡

⎤ j j

Cg exp Eb /kT ⎥

Eb ⎢ ξ K0 F(η ) max i ⎢ ⎥

1+ exp Ef /kT CP = Cg ⎣ , (6.62) Ef ∑ C j exp E j /kT ⎦ ADk2 g b j

where Cg is the total impurity concentration in the grain, Ebj is the binding energy between the point defect, the self-interstitial and the impurity atom, Ef is the interstitial formation energy and Cgj is the concentration of impurity atom, j in the grains. The denominator of the first bracket is the sum of point defect binding energy terms for all of the elements entering into the site competition process. In the second bracket, ξ is the defect production efficiency, F(η ) is a recombination term, K0 is the defect production rate, A is associated with the vibrational entropy of the atoms surrounding the point defect, D is the defect diffusion coefficient, and k2 is the sink efficiency. Following segregation to the boundary, the impurity concentration will be determined by site competition at the boundary where the concentration of phosphorus is given by: CP∗ = CPmax

CgP exp(QP /kT ) Cgj exp(Q j /kT ) + CgP exp(QP /kT )

,

(6.63)

j

where CgP is the concentration of P and Cg is the concentration of the other impurity elements in the grains, and QP and Q j are the solute grain boundary binding energies for P and for the other elements, respectively. The value of CP∗ is the maximum expected segregation at steady state. Before steady state is reached, the grain boundary concentration depends on time according to: √ CP (t) − Cg 4Dct 2 Dc t = 1 − exp erfc , (6.64) CP∗ − Cg α 2d2 αd where Dc is the point defect–impurity complex diffusion coefficient, α is the enrichment ratio and d is the grain boundary width. Experimental measurements of P segregation in ferritic steels are shown in Fig. 6.17. Note that while the P concentration increases with dose, it varies significantly with the specific alloy. This variation is likely due to site competition with other impurities, most important of which is carbon. The A533 B steel shown has a high grain boundary P level because it has a low C content. Figure 6.18 shows the competition between P and C at the grain boundary and the P segregation is highest when the C level is low.

6.6 RIS in Ferritic Alloys

261

Fig. 6.17. Dose dependence of the irradiation-induced change in grain boundary phosphorus monolayer coverage normalized with respect to the bulk atomic phosphorus concentration for C-Mn LWR plates, welds and coarse HAZ structure and VVER base metal and weld. All irradiation temperatures are 275 – 290 ◦C except for the Magnox SAWs, which cover the range 186 – 311 ◦C (after [21])

In the higher Cr alloys such as the 9–12%Cr ferritic-martensitic alloys, the behavior of Cr at the grain boundary is of concern because of the potential for the formation of brittle, chromium-rich phases. While Cr depletes in austenitic alloys, recent results have shown that it enriches in F-M alloys, behaving like an undersize solute [22]. Although this behavior is not yet understood, experiments have indeed shown that enrichment of Cr at the grain boundary can be substantial. Figure 6.19 shows that Cr enriches at the grain boundary of a Fe–9Cr alloy (T91) by almost 5 wt% following irradiation with 2 MeV protons to 10 dpa at 450 ◦C. If such enrichment leads to the formation of Cr-rich phases, grain boundary embrittlement could result.

262

6 Radiation-Induced Segregation

Fig. 6.18. Variation of phosphorus and carbon monolayer coverage at grain boundaries of thermally aged and irradiated ferritic alloys (after [21])

Fig. 6.19. Grain boundary composition of a ferritic-martensitic Fe–9Cr steel containing 0.2%V and irradiated with 2 MeV protons at 450 ◦C to 10 dpa (after [22])

Nomenclature

Nomenclature A Cx CP∗ d dxy d0x D Dyx x Eeq Ebxz Efx xz Em Exy ord Exy x ESalloy f F(η ) i k k2 v s Jx K0 Kxy Mj Nx QS j rxy R x Sm t T z

Term associated with vibrational entropy, see Eq. (6.62) Concentration of specie x Maximum grain boundary segregation of P at steady state in ferritic steels Grain size Partial diffusion coefficient divided by Ny Pre-exponential term for diffusion of specie x Diffusion coefficient Partial diffusion coefficient for migration of x via y Equilibrium energy for specie x Binding energy of specie x to defect z Formation energy of specie x Migration energy of specie x migrating via defect z Interaction energy between species x and y Ordering energy for species x and y Saddle point energy for element x in alloy Correlation coefficient Recombination term in Eq. (6.62) Interstitial designation Boltzmann’s constant Sink efficiency Vacancy designation Sink designation Flux of atom or defect x across a marker plane Defect production rate Reaction rate constant for x and y Determinant for specie j (defined in Eqs. (6.23) and (6.39)) Atom fraction of specie x Grain boundary binding energy for solute j Capture radius for defect x by sink/trap y Recombination rate Entropy of migration for specie x Time Temperature Number of nearest neighbors

α γx κxy λ ω Ω

Enrichment ratio Activity coefficient of specie x Capture coefficient of defect x by sink/trap y Jump distance Jump frequency Atomic volume

263

264

6 Radiation-Induced Segregation

τ ξ

Time constant Defect production efficiency

Subscripts eq f g l m

Equilibrium Formation Impurity Trap type Migration

Superscripts j k ord t

Specie or defect solute Ordering Trap

Acronyms AES BWR F-M IASCC IGSCC IGC IK MIK MIK-T RIS STEM-EDS

Auger electron spectroscopy Boiling water reactor Ferritic-martensitic Irradiation assisted stress corrosion cracking Intergranular stress corrosion cracking Intergranular cracking Inverse Kirkendall Modified inverse Kirkendall Modified inverse Kirkendall-trapping Radiation-induced segregation Scanning transmission electron microscopy-energy dispersive spectrometry

Problems 6.1 A sample of Cu–20%Al is irradiated at 500 ◦C. a) Will aluminum segregate to or from the surface? Explain. (Assume that association of defects with Al and Cu atoms is non-preferential.) b) If there is strong binding (a preferential association) of interstitials to the undersized atom, how would your answer to part (a) change? (Take EbCu-i = 1 eV.) c) Repeat part (a) for T = 100 ◦C. (Here, vacancies are immobile.) 6.2 A Ni–18Cr alloy is irradiated at 400 ◦C. a) The chromium concentration is measured at the grain boundary and is found to deplete. What is the sign of the determinant for chromium?

References

265

b) The bulk concentration of nickel decreases from 82 to 70 wt%. Assuming nothing else changes, what happens to the determinant of chromium? State your assumptions. c) If the diffusion coefficient of chromium vacancies decreases, what happens to the Cr segregation profile? 6.3 An Fe–18Cr–8Ni alloy is irradiated and radiation-induced segregation changes the grain boundary composition. Calculate the Ni and Cr equivalents for the bulk alloy and at the grain boundary assuming ΔCr = −5 and ΔNi = +3. In terms of the Schaeffler diagram, how is the grain boundary area different than the bulk? If an Fe–18Cr–20Ni alloy was irradiated under the same conditions, what changes? 6.4 For the ternary alloy Fe–18Cr–20Ni, determine if iron enriches or depletes during irradiation at 500 ◦C. 6.5 For the Fe–18Cr–20Ni alloy in Problem 6.4, determine the migration enCr-v at the grain boundary when the grain ergy for chromium via vacancies, Em boundary composition is Fe–10Cr–30Ni. Cr Ecoh = −4.10 eV Fe Ecoh = −1.28 eV Ni Ecoh = −4.44 eV

EfCr-v = 1.60 eV EfFe-v = 1.40 eV EfNi-v = 1.79 eV ord = 0.005 eV ENiCr ord = 0.003 eV EFeCr

References 1. Bruemmer SM, Simonen EP, Scott PM, Andresen PL, Was GS, Nelson LJ (1999) J Nucl Mater 274:299–314 2. Anthony TR (1972) In: Corbett JW, Ianniello LC (eds) Radiation-Induced Voids in Metals and Alloys, AEC Symposium Series, Conf-701601, p 630 3. Okamoto PR, Harkness SD, Laidler JJ (1973) ANS Trans 16:70 4. Wiedersich H, Okamoto PR, Lam NQ (1979) J Nucl Mater 83:98–108 5. Perks JM, Marwick AD, English CA (1986) AERE R 12121 (June) 6. Rehn LE, Okamoto PR, Potter DI, Wiedersich H (1978) J Nucl Mater 74:242–251 7. Rehn LE (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier Science, New York, p 17 8. Okamoto PR, Wiedersich H (1974) J Nucl Mater 53:336–345 9. Kornblit L, Ignatiev A (1984) J Nucl Mater 126:77–78 10. Was GS, Allen TR, Busby IT, Gan I, Damcott D, Carter D, Atzmor M, Konik EA (1999) J Nucl Mater 270:96–114

266

6 Radiation-Induced Segregation

11. Was GS, Allen TR (1993) J Nucl Mater 205:332–338 12. Allen TR, Was GS (1998) Acta Metal 46:3697 13. Lam NQ, Kumar A, Wiedersich H (1982) In: Brager HR, Perrin JS (eds) Effects of Radiation on Materials, 11th Conference, ASTM STP 782, American Society for Testing and Materials, pp 985–1007 14. Watanabe S, Takahashi H (1994) J Nucl Mater 208:191 15. Grandjean Y, Bellon P, Martin G (1994) Phys Rev B 50:4228 16. Nastar M, Martin G (1999) Mater Sci Forum 294–296:83 17. Mansur LK, Yoo MH (1978) J Nucl Mater 74:228–241 18. Hackett MJ, Was GS, Simonen EP (2005) J ASTM Int 2(7) 19. Fournier L, Sencer BH, Wang Y, Was GS, Gan J, Bruemmer SM, Simonen EP, Allen TR, Cole JI (2002) In: Proceedings of the 10th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, NACE International, Houston, TX 20. Was GS (2004) Recent developments in understanding irradiation assisted stress corrosion cracking. In: Proceedings of the 11th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, American Nuclear Society, La Grange Park, IL, pp 965–985 21. Faulkner RG, Jones RB, Lu Z, Flewitt PEJ (2005) Phil Mag 85(19):2065–2099 22. Gupta G, Jiao Z, Ham AN, Busby JT, Was GS (2006) J Nucl Mater 351(1–3):162–173

7 Dislocation Microstructure

One of the most profound consequences of irradiation on the microstructure of materials is the formation of dislocation loops. Dislocation loops have a bias for interstitials and thus have a strong impact on the development of the irradiated microstructure. They also influence the deformation behavior and consequently, the ductility and hardening of irradiated materials, as will be discussed in Chap. 12. In this chapter, we will review the origin and character of dislocations, their mobility and multiplication and their stresses, strains and energies. The character of dislocation loops will be examined and models for nucleation and growth will be presented. Finally, the stacking fault tetrahedron will be discussed. For a more in-depth treatment of dislocations, the reader is referred to [1, 2, 3, 4].

7.1 Dislocation Lines The discovery of dislocations in crystals has its origin in the discrepancy between the measured and theoretical stress needed to cause shear in a crystal. Consider the stress required to shear a crystal along a given atomic plane. A shear of one atomic distance requires that atoms above the plane all move one lattice spacing relative to those below (Fig. 7.1). To reach the saddle point, each atom must move horizontally a distance of one atom radius, a. Since the separation of two planes is ∼ 2a, the shear strain at the saddle point is γ ≈ a/2a ∼ 1/2. In a perfectly elastic crystal, the ratio of shear stress to shear strain is the shear modulus: σs =μ. (7.1) γ

Fig. 7.1. Initial position of atoms above and below a slip plane, and the motion of the atoms above the slip plane required to cause slip

268

7 Dislocation Microstructure

For a typical shear modulus of 17 GPa and a shear strain of 1/2, the shear stress from Eq. (7.1) is ∼ 8.5 GPa. However, experiments, for example on magnesium, produce deformation at shear stresses of ∼ 1 MPa, which is different from theory by a factor of 104 ! The reason is the existence of dislocations that provide for much reduced shear stresses in crystals. A dislocation is a line that forms a boundary between a region of the crystal that has slipped and one that has not. The two basic types of dislocations lines are the edge and the screw. In an edge dislocation, atoms over the cut surface are shifted in a direction perpendicular to the dislocation line. An edge dislocation can also be thought of as the insertion of an extra half plane of atoms (Fig. 7.2). In a screw dislocation, the atoms over the cut surface are shifted in a direction parallel to the dislocation line (Fig. 7.3a). The screw dislocation itself is a pole about which a spiral ramp of planes circles (analogous to a parking garage ramp) (Fig. 7.3b). There also exist mixed dislocations in which the shift is neither parallel nor perpendicular to the dislocation line, but at some arbitrary angle. Figure 7.4 shows a mixed dislocation in a crystal in which the dislocation line is curved. Note that the boundary separating slipped and unslipped regions is circular. At point A (front face), the dislocation is of pure edge character. At point B (side face), the dislocation is of pure screw character. In between, the dislocation is mixed with the proportion of screw and edge character varying continuously with distance along the line. Figure 7.5 shows the construction of a mixed dislocation.

Fig. 7.2. An edge dislocation described as an extra half plane of atoms above the slip plane

Fig. 7.3. (a) A screw dislocation formed by a cut and a shift of atoms in a direction parallel to the cut line. (b) A schematic showing the “parking ramp” nature of a screw dislocation in which atom planes spiral about the dislocation line

7.1 Dislocation Lines

269

Fig. 7.4. Curved dislocation line with pure screw character at point A, pure edge character at point B and mixed character along the length of the dislocation

Fig. 7.5. Construction of a dislocation line with mixed character

270

7 Dislocation Microstructure

Fig. 7.6. A perfect dislocation loop in a crystal in which the character of the loop varies with position long the loop

A dislocation line can also be made in the form of a closed loop rather than a line that terminates at the crystal surface. Following Fig. 7.6, we make a cut along ABCD and shift the atoms parallel to the plane and then rejoin them. Note that segments AB and DC have edge character and segments BC and AD have screw character. Segments AB and DC have opposite sign in that one has a half plane above the cut and one has the half plane below it. The same is true with segments BC and AD. This loop is termed a perfect dislocation loop. Now suppose that instead of shifting atoms parallel to the plane as we did in the example of a perfect loop, we fill up the cut with more atoms. The shift of atoms on each side of the cut is perpendicular to the surface. Figure 7.7 shows that by insertion of a disk of atoms into the cut, that every segment of the dislocation loop has pure edge character. This is very different from the perfect loop with edge and screw character. This dislocation loop is called a prismatic or Frank loop. One variation is to remove a disk of atoms from the cut rather than insert an extra plane of atoms. 7.1.1 Dislocation Motion Dislocations can move in two modes: glide and climb. Glide is the motion of a dislocation on its slip plane and is conservative motion in that it requires no long-range mass transport in order to occur. Experiments have shown that the logarithm of the dislocation velocity is proportional to the logarithm of the shear stress causing glide: ln g α ln σs ,

(7.2)

which implies a power law relationship between shear stress and dislocation velocity: m σs g = , (7.3) σD

7.1 Dislocation Lines

271

Fig. 7.7. A Frank dislocation loop formed by insertion of a circular plane of atoms between existing planes in the lattice

where m is the stress exponent (∼ 1.65) and σD is the value of the stress that yields a dislocation velocity of 0.01 m/s [5]. Experiments also show that the logarithm of the dislocation velocity is proportional to the reciprocal of the absolute temperature, T : ln g α

1 , T

(7.4)

leading to the following description of the velocity of a gliding dislocation in terms of stress and temperature: g = f (σ ) exp(−E/kT ) .

(7.5)

When dislocations glide, they displace the crystal above the slip plane relative to that below. Figure 7.8 shows that if an edge dislocation glides to the surface, the result is a step on the surface of magnitude equal to the Burgers vector. Screw dislocations will also produce a step on the surface, but on a face that is perpendicular to the dislocation line (Fig. 7.9). The perfect loop described in the last section will also

272

7 Dislocation Microstructure

Fig. 7.8. Slip produced by movement of edge dislocations to the surface of a crystal

Fig. 7.9. Slip produced by movement of a screw dislocation to the surface of a crystal

result in displacement of the crystal when it reaches the surface. Figure 7.10 shows the displacement of the crystal above the slip plane relative to that below. Note that the displacements are entirely consistent with the character of the dislocation where it intersects the surface as shown in Figs. 7.8 and 7.9. A Frank loop is essentially an edge dislocation. The slip plane for this type of loop is defined by the intersection of the loop edge and the adjacent crystal and consists of a cylindrical surface projecting above and below the plane of the loop. Figure 7.11 shows how surface atoms would be displaced if the loop were to glide to the surface. However, this mode of motion is not energetically favorable and this loop is more likely to move by climb rather than glide. Dislocations also move by a non-conservative process called climb. Climb is an important process for edge dislocations and prismatic loops, since unlike screw dislocations that can glide on any plane containing the dislocation, there is only

Fig. 7.10. Slip produced by movement of a perfect dislocation loop to the surface of a crystal

7.1 Dislocation Lines

273

Fig. 7.11. Slip produced by movement of a Frank loop to the surface of a crystal

one possible slip plane for an edge dislocation to glide. Climb is the extension or recession of the extra half plane of atoms by absorption or emission of a vacancy, absorption of an interstitial atom or emission/absorption of clusters of vacancies or SIAs. Figure 7.12 shows the positive climb of an edge dislocation by absorption of a vacancy at the dislocation core. In order for the edge dislocation to move up one lattice spacing, all of the atoms along the edge (into the paper) must absorb a vacancy. Positive climb results in a decrease in the size of the extra half plane, while negative climb results in the increase in the size of the extra half plane. Positive climb is associated with a compressive strain and will be promoted by a compressive stress component perpendicular to the extra plane. Similarly, a tensile stress applied perpendicular to the extra plan promotes growth of the plane and thus, negative climb. Since they are essentially edge dislocations, Frank loops climb in the same manner, where positive climb results in loop shrinkage and negative climb results in loop growth. Note that there is a fundamental difference between the nature of the stress that produces slip and that which produces climb. Slip occurs as the result of shear stress, and climb occurs as a result of a normal stress. Since climb requires that vacancies move through the lattice either to or away from the extra half plane, the rate of climb will be dependent on both the diffusion coefficient of vacancies and their concentration. In unirradiated solids, this means that climb will be most important at high temperature. However, in irradiated solids, the increased population of vacancies will make climb more important at lower tem-

Fig. 7.12. Positive climb of an edge dislocation by absorption of vacancies at its core

274

7 Dislocation Microstructure

peratures. Further, the elevated concentration of interstitials means that they too can contribute to climb in a direction that is opposite to that of vacancies. 7.1.2 Description of a Dislocation A description of a dislocation consists of the specification of the vector defining the line direction, s and the Burgers vector defining the atom shift, b. The Burgers vector is defined as follows: 1. Define a positive direction, s, along the dislocation line (e.g., into the paper). 2. Construct a plane perpendicular to the dislocation line. 3. Starting in a region of perfect crystal (away from the dislocation core), complete a counterclockwise circuit around the dislocation line (in the plane of the paper) 4. The Burgers vector, b is the vector needed to close the circuit. The rule is shown schematically in Fig. 7.13 for a screw dislocation. Following this convention, the Burgers vector of an edge dislocation is perpendicular to the dislocation line. The Burgers vector of a screw dislocation is parallel to the dislocation line. For an edge dislocation, we can determine the Burgers vector in the following manner. Sighting down the dislocation line (along the positive s direction), we make a counterclockwise circuit around the dislocation. The vector connecting the end point to the origin is the Burgers vector. Figure 7.14 shows an example of the determination of the Burgers vector using the construction rule. (Note that it does not matter which direction is called positive, but we need to adopt a convention in order to determine the orientation of the line and the extra half plane in the crystal. If we sighted in the opposite direction, b will be in the opposite direction. What matters is the specification of s relative to b.) Following the convention, Fig. 7.15a shows a dislocation with line direction, s pointing into the paper and b pointing to the left. The dislocation in Fig. 7.15b is identical to that in Fig. 7.15a since the relationship between s and b is the same. However, the dislocation shown in Fig. 7.15c is of opposite sign. For a screw dislocation, we consider a left handed screw (counterclockwise rotation; see Fig. 7.16). With this convention, s and b are in the same direction. Figure 7.17a shows a screw dislocation with Burgers vector in the same direction as s.

Fig. 7.13. Convention for finding the Burgers vector of a dislocation line characterized by direction s

7.1 Dislocation Lines

275

Fig. 7.14. The Burgers circuit for an edge dislocation following the convention shown in Fig. 7.13

Fig. 7.15. Examples of identical edge dislocations (a) and (b) and an edge dislocation of opposite sign (c)

Fig. 7.16. The Burgers circuit for a screw dislocation following the convention shown in Fig. 7.13

The dislocation shown in Fig. 7.17b is identical to that in Fig. 7.17a, but the dislocation shown in Fig. 7.17c is of opposite sign as the other two. An edge dislocation glides in the direction of its Burgers vector. A screw dislocation glides in a direction perpendicular to its Burgers vector. We adopt the following convention to determine the direction of motion of a dislocation line: The positive direction of motion is obtained by a counterclockwise rotation on a plane parallel

276

7 Dislocation Microstructure

Fig. 7.17. Examples of identical screw dislocations (a) and (b), and a screw dislocation of opposite sign (c)

to the slip plane, and through 90◦ from the positive direction of the dislocation line itself. The rule is shown by the illustration in Fig. 7.18a. Figures 7.18b,c show the positive direction of motion for an edge and screw dislocation, respectively. Figure 7.19 shows the direction of motion for a dislocation loop that is characterized by a single Burgers vector (perfect loop) and changes character along the dislocation line. 7.1.3 Displacements, Strains and Stresses Dislocations interact with each other and with other microstructure features through their stress fields. Therefore, it is important to establish the stress and strain fields around a dislocation as well as the energy associated with the dislocation line. We will begin with the screw dislocation and then treat the edge dislocation. Recall the orientation of the screw dislocation is one in which the Burgers vector is parallel to the dislocation line, which means that the displacement of atoms is in the direction of the dislocation line. If we describe the dislocation in cylindrical coordinates, Fig. 7.20, then there is no displacement along the r or θ directions so that: ur = uθ = 0 .

(7.6)

In Cartesian coordinates, the displacement in the x–y plane is zero. The only displacement is in the z-direction, and from inspection, we have in cylindrical coordinates: uz =

b θ, 2π

ur = uθ = 0 ,

(7.7)

and in Cartesian coordinates: uz =

y b tan−1 , 2π x

(7.8)

where b is the magnitude of the Burgers vector. From elasticity theory, we can calculate the strain from the displacement as: 1 εθ z = r

∂ uz ∂θ

=

b , 2π r

εrr = εθ θ = εzz = εrθ = εrz = 0 ,

(7.9)

7.1 Dislocation Lines

277

Fig. 7.18. (a) Rule for determination of the direction of motion of a dislocation on its slip plane and examples of the positive direction of motion for (b) edge and (c) screw dislocations

and in Cartesian coordinates: y b b sin θ = 2 π x2 + y2 2 π r x b b εyz = − cos θ =− 2 π x2 + y2 2π r εxx = εyy = εzz = εxy = 0 .

εxz =

(7.10)

278

7 Dislocation Microstructure Fig. 7.19. Positive direction of motion of a perfect loop characterized by a single Burgers vector

Fig. 7.20. Screw dislocation in the Cartesian coordinate system

The stress field of the screw dislocation is determined from the relation between stress and strain: μb , σrr = σθ θ = σzz = σrθ = σrz = 0 , σθ z = μεθ z = (7.11) 2π r and: μb y μb sin θ σxz = = 2 π x2 + y2 2π r μb x μb (7.12) σyz = − cos θ =− 2 2 2π x + y 2π r σxx = σyy = σzz = σxy = 0 . For an edge dislocation as shown in Fig. 7.21, the displacement of atoms is in the x-direction. The displacement is not so simple here, but we know that the dislocation will be similar at any point along the z-axis and hence, the stress state is one of plane stress. The displacement field around the edge dislocation in Cartesian coordinates is:

λ + μ xy b −1 y ux = + tan 2π x λ + 2 μ x2 + y2

−μ x2 + y2 λ +μ y2 b (7.13) uy = log + 2π 2(λ + 2μ ) c λ + 2 μ x2 + y2 uz = 0 ,

7.1 Dislocation Lines

279

Fig. 7.21. Edge dislocation in the Cartesian coordinate system

where the constant c is added to make the log term dimensionless, but is irrelevant since stresses and strains are derivatives of the displacements. The resulting strains are:

εxx = − εyy =

by μ y2 + (2λ + 3μ )x2 2π (λ + 2μ )(x2 + y2 )2

by (2λ + μ )x2 − μ y2 2π (λ + 2μ )(x2 + y2 )2

(7.14)

x(x2 − y2 )

b 2π (1 − ν ) (x2 + y2 )2 εzz = εxz = εyz = 0 ,

εxy =

where ν is Poisson’s ratio, λ is the Lam´e constant and ν = around an edge dislocation are then:

σxx =

λ . The stresses 2(λ + μ )

−μ b y(3x2 + y2 ) −μ b sin θ (2 + cos2θ ) = 2π (1 − ν ) (x2 + y2 )2 π (1 − ν )r

y(x2 − y2) μb μb sin θ cos 2θ = 2π (1 − ν ) (x2 + y2)2 π (1 − ν )r μb μb x(x2 − y2 ) cos θ cos 2θ = σxy = − 2π (1 − ν ) (x2 + y2 )2 π (1 − ν )r −2 μν b μν by = sin θ σzz = v(σxx + σyy ) = π (1 − ν )(x2 + y2 ) π (1 − ν )r σxz = σyz = 0 .

σyy =

(7.15)

280

7 Dislocation Microstructure

The stresses in cylindrical coordinates are: sin θ μb 2π (1 − ν ) r −μ b cos θ σrθ = 2π (1 − ν ) r −μν b sin θ σzz = 2π (1 − ν ) r σθ z = σrz = 0 .

σrr = σθ θ =

(7.16)

7.1.4 Energy of a Dislocation Energy is stored in any elastic medium that is stressed. Applying a tensile stress to a rod produces a tensile strain, which is proportional to the stress in an elastic solid. Consider a unit cube within the rod. A stress, σ is the total force applied across a face of the cube. The strain is the fractional distance the cube elongates in the direction of the stress. So the work done (energy/unit volume) on the cube is the force times the distance, or: W=

εmax 0

σ dε ,

(7.17)

and from Fig. 7.22, we have: W = 1/2σmaxεmax .

(7.18)

For a generalized stress field, the stored energy per unit volume is: W = 1/2(σxx εxx + σyy εyy + σzz εzz + σxy εxy + σxz εxz + σyz εyz ) ,

(7.19)

and in cylindrical coordinates: W = 1/2(σrr εrr + σθ θ εθ θ + σzz εzz + σrθ εrθ + σrz εrz + σθ z εθ z ) ,

(7.20)

where σi j = σ ji .

Fig. 7.22. Elastic stress-strain curve showing the stored energy in the strain field

7.1 Dislocation Lines

281

Applying Eq. (7.20) to the screw dislocation gives: W = 1/2(σθ z εθ z ) =

μ b2 . 8π 2 r 2

The elastic energy per unit length of the dislocation line is: R R μ b2 R dr μ b2 = W 2π r dr = ln + εc . El = 4 π r 4 π r rc rc c

(7.21)

(7.22)

The limits on the integral are the dislocation core radius, rc , and R. The dislocation core radius is that distance below which linear elasticity does not hold and is generally taken to be several Burgers vectors in magnitude. R is the outer dimension of the crystal, or for polycrystalline materials, R could be taken to be the grain radius. However, a further constraining condition is the presence of other dislocations, which is the case even in a well-annealed metal in which the dislocation density is still ∼ 108 cm−2 . So R is often taken to be the distance midway to the next dislocation. However, the elastic energy is not highly sensitive to R since it appears in the ln term. The term εc is the energy of the dislocation core radius, which is not included in the integral since linear continuum elasticity theory breaks down in this region. Assuming that the stress level in the core is μ /30, then for a dislocation core radius of 5b, the value of εc is approximately μ b2 /10, which is about 10 – 20% of the value of that in the elastic strain field (ln term). For an edge dislocation, the elastic energy per unit length determined in the same way as for the screw dislocation is: R μ b2 ln (7.23) + εc , El = 4π (1 − ν ) rc which is different from the screw dislocation by a factor of (1 − ν ) in the denominator of the first term, or a factor of about 1.6 for ν ∼ 0.3. For typical values of R and rc , μ b2 ≤ El ≤ μ b2 . The elastic energy per unit length of dislocation line is also called 2 μ b2 . the line tension and is denoted by Γ . Generally, Γ is taken to have the value 2 7.1.5 Line Tension of a Dislocation Under a uniform applied shear stress, σs , an element of dislocation line, ds, is displaced in a direction normal to ds by an amount dl (Fig. 7.23). The area swept out by the dislocation line element, ds, is ds dl. The average displacement of the crystal above the slip plane relative to that below is by an element: ds dl dx = b, (7.24) A

282

7 Dislocation Microstructure Fig. 7.23. Dislocation line segment ds sweeping out an area ds dl in the direction of the Burgers vector

where A is the area of the slip plane. The force creating the shear stress is σs A, and the work done is: ds dl dW = F dx = σs A b A (7.25) = σs ds dlb . Since force is work divided by the distance over which it is applied: F=

dW = σs dsb , dl

(7.26)

and the force per unit length is: Fl =

dW / dl = σs b . ds

(7.27)

Consider a curved dislocation line. The line tension produces an inward radial force that tends to straighten out the dislocation line. The dislocation will only remain curved if a shear stress exists to resist the line tension. We wish to determine the shear stress required to maintain the curvature. Consider a segment of a dislocation line as shown in Fig. 7.24. The outward force due to the shear stress is:

σs b ds = 2σs bR dθ .

(7.28)

Fig. 7.24. Inward restraining force on a dislocation line segment ds due to a shear stress σs

7.1 Dislocation Lines

283

The inward restraining force is:

Γ sin( dθ ) ∼ 2Γ dθ .

(7.29)

From Eqs. (7.28) and (7.29) we have the force balance: 2Γ dθ = 2σs bR dθ ,

(7.30)

and solving for σs yields the shear stress in terms of the line tension:

σs =

Γ . bR

(7.31)

For:

Γ≈

μ b2 , 2

then σs =

μb , 2R

(7.32a)

and for

μb . (7.32b) R One mechanism of formation of dislocations in solids is the Frank–Read mechanism. The mechanism is shown in Fig. 7.25 and occurs as follows. A dislocation line segment defined by ABCD and Burgers vector b is such that segments AB and DC are immobile and only segment BC lies in a slip plane. The dislocation segment BC is pinned at the points B and C. The temperature is assumed to be low enough that that climb is not an option. Under an applied stress, the segment BC bows out slightly in response to the stress and adopts the curvature as prescribed by μb the line tension on the dislocation given in Eq. (7.32b) σs = , and for l = 2R, 2R μb . When the force arising from the curvature of the dislocation line can no σs ≈ l longer balance the force produced by the applied stress, becomes unstable and bows out to adopt the configuration shown in Fig. 7.25c. Note that at this point, the line segments P and P have opposite character and as the dislocation continues to bow out they come in contact with each other and annihilate, leaving a region of perfect crystal and a perfect loop. The applied shear stress will cause the loop to expand and will also start the process of creating a new loop from the same BC segment. This process can continue to occur and one such pinned dislocation can produce many loops and will continue as long as the loops are able to expand away from the source. Figure 7.26 shows a micrograph of a Frank–Reed source in a silicon crystal. Eventually, the back stress caused by the previous loops will produce a retarding force on the source and it will shut down. Back stress due to dislocation pileup is discussed in Chap. 12. Γ ≈ μ b2 ,

then σs =

7.1.6 Forces on a Dislocation Application of a shear stress, σxy , on a solid containing an edge dislocation (Fig. 7.27) produces motion in the +x direction. In moving a dislocation a distance L, the external applied stress will have done an amount of work/unit length of

284

7 Dislocation Microstructure

Fig. 7.25. Frank–Read source for the production of dislocations

Fig. 7.26. Micrograph of a Frank–Read source in a silicon crystal (from [6])

Fig. 7.27. Force on an edge dislocation with character s|001|, b|100| due to a shear stress σxy

7.1 Dislocation Lines

285

dislocation line equal to σxy bL. Then the force is F = σxy b. Note that the force is in the +x direction. For a screw dislocation, application of a shear stress, σyz , results in a force σyz b, where the force is in the +x direction (Fig. 7.28). Application of a shear stress σxz produces a force −σxz b, where the force is in the −y direction, and motion is perpendicular to the slip plane. What if we apply a stress to an edge dislocation that produces a force in a direction perpendicular to the slip plane? A tensile stress, σxx , applied to the edge dislocation in Fig. 7.29 will produce a downward force on the dislocation equal to −σxx b. The only way that the dislocation can respond to this stress is to climb. Forces on mixed dislocations are more complicated. If a dislocation is oriented along the +z-direction and its slip plane is perpendicular to the y-axis, then the Burgers vector can be described by: b = bx i + bz k ,

(7.33)

Fig. 7.28. Force on a screw dislocation with character s|001|, b|001| due to a shear stress σyz

Fig. 7.29. Force on an edge dislocation with character s|001|, b|100| due to a normal stress σxx

286

7 Dislocation Microstructure

where bx and bz are edge and screw components of the Burgers vector and i and k are unit vectors in the x and z-directions, respectively. An external stress placed on the surfaces of a crystal containing a dislocation includes six components; σxx , σyy , σzz , σxy , σxz and σyz . Of these six stress components, only σyz and σxy can exert a force on an edge dislocation that will cause motion in the slip plane. Stress components σxz and σxx causes motion perpendicular to the slip plane. The term σzz does no work, nor does σyy . The total force on a unit length of dislocation line is then: F = (σxy bx + σyz bz )i − (σxx bx + σxz bz )j ,

(7.34)

where the first term is the force component parallel to the slip plane and the second term is the force component normal to the slip plane, and n = (i, j, k) defines the unit vector. As an example of forces between dislocations, let us take the case of parallel screw dislocations. The force, F that a screw dislocation situated at the origin (with Burgers vector b) exerts on a parallel screw dislocation at a position (r, θ ) (with Burgers vector b ) is: F = σyz bz · i − σxz bz · j μ br cos θ μ br sin θ b+ b = 2π r 2 2π r 2 μ bb r = (cos θ · i + sin θ · j) . 2π r 2

(7.35)

The force is in a direction that is perpendicular to the dislocation lines. It is repulsive if the dislocations are of the same sign, and attractive if the dislocations are of opposite sign. The force on the dislocation at the origin due to the dislocation at (r, θ ) is equal in magnitude but opposite in sign from the force on the dislocation at (r, θ ) due to that at the origin. The force components in the xy-plane are shown in Fig. 7.30a and the magnitude of the forces as a function of θ are shown in Fig. 7.30b. A dislocation of mixed character represents the generalized case of a force on a dislocation. For a mixed dislocation, the Burgers vector is: b = bx i + by j + bz k = b1 i + b2 j + b3 k .

(7.36)

Therefore, we write the incremental work done on a dislocation of Burgers vector described by Eq. (7.36) due to an arbitrary stress σi j , as:

δW =

3

∑ bi σi j n j dA ,

(7.37)

i=1 j=1

or in matrix notation: dW = b σ n dA ,

(7.38)

7.1 Dislocation Lines

287

Fig. 7.30. The x and y-components of the force on a screw dislocation due to another dislocation (a) in the x–y plane, and (b) as a function of θ

where σ is the stress tensor, n is the unit vector perpendicular to the slip plane and b is the Burgers vector. Actually, b is a column vector so that Eq. (7.38) is written as: dW = bT σ · n dA .

(7.39)

The term n dA can be written as dA which is just L(s × dl) ,

(7.40)

where s is the unit vector in the direction of the dislocation line, L is the length of the dislocation line and dl (= dxi + dyj + dzk) is the unit vector in the slip plane and is normal to s and n. Recall that b = bx i + by j + bz k, so b has a component only in the direction dl. Since A · B × C = A × B · C, then: dW = bT σ × s · dlL ,

(7.41)

and: 1 dW = bT σ × s · dl . L

(7.42)

288

7 Dislocation Microstructure Fig. 7.31. Orientation of an edge dislocation for the determination of the forces due to a generalized stress field

The term bT σ × s in Eq. (7.42) is the force per unit length on a dislocation due to an external stress which tends to displace the dislocation, and is designated: f = bT σ × s ,

(7.43)

and is known as the Peach–Koehler equation. Let us apply the Peach–Koehler equation to the case of an edge dislocation described vector and direction: Burgers by 0 1 b 0 and s 0 and shown in Fig. 7.31. We write the first quantity in Eq. (7.43) 1 0 as: σxx σxy σxz bT σ = b|100| σyx σyy σyz = b|σxx σxy σxz | , (7.44) σzx σzy σzz and then taking the cross product with s gives: i j k bT σ × s = b σxx σxy σxz . 0 0 1

(7.45)

The cross product, or determinant is bσxy i − bσxx j, and the force on the dislocation is: f = bσxy i − bσxx j .

(7.46)

Note that fx = bσxy is a glide force in the +x-direction and the force component fy = −bσxx is the climb force in the −y-direction. Only σxy and σxx can exert forces on a dislocation with Burgers vector and direction defined as in this example. For with Burgers vector and direction given by: ascrew dislocation 0 0 b 0 and s 0 , and shown in Fig. 7.32, we have: 1 1

7.1 Dislocation Lines

289

Fig. 7.32. Orientation of a screw dislocation for the determination of the forces due to a generalized stress field

σxx σxy σxz bT σ = b|001| σyx σyy σyz = b|σxz σyz σzz | , σzx σzy σzz and then taking the cross product with s gives: i j k f = bT σ × s = b σxz σyz σzz = bσyz i − bσxz j , 0 0 1

(7.47)

(7.48)

and fx = bσyz and fy = −bσxz . Note that only σyz and σxz can exert a force on a dislocation defined in this example. 7.1.7 Interactions Between Dislocations Let us examine interactions between dislocations. We will look at edge–edge, screw–screw, and edge–screw interactions. We will begin with the edge–edge interaction. Edge–edge interaction To find the force on dislocation (2) due to the presence of dislocation (1), we locate dislocation (1) at the origin of our coordinate axes and dislocation (2) at some arbitrary position (Fig. 7.33a). According to the Peach–Koehler equation, the force is: f = b T σ × s , where the Burgers vector and direction are those of disloca(2) (1)

(2)

tion (2), and the stress is due to dislocation (1). The first term in the cross product then becomes: σxx σxy 0 bT σ = b|100| σyx σyy 0 = b|σxx σxy 0|; , (7.49) % &' ( 0 0 σ zz (2) % &' ( (1)

290

7 Dislocation Microstructure

Fig. 7.33. (a) Orientation of dislocations to determine the force on edge dislocation (2) due to edge dislocation (1), and x and y-components of the force (b) in the x–y plane, and (c) as a function of θ

and

i j k f = bT σ × s = b σxx σxy 0 = bσxy i − bσxx j . (2) 0 0 1

(7.50)

The force on dislocation (2) can be written as: F=

μ bb(2) μ bb(2) (cos θ cos2θ )i − sin θ (2 + cos2θ )j , 2π (1 − ν )r 2π (1 − ν )r &' ( % &' ( % Fx (θ )

(7.51)

Fy (θ )

and the force components in the x–y plane are shown in Fig. 7.33b, and as a function of θ in Fig. 7.33c. Note that if dislocation (2) has the same s but the Burgers vector is in the opposite direction, then the net effect on the resultant force is simply a change in sign of

7.1 Dislocation Lines

291

each of the terms in Eq. but preservation of the magnitudes. If dislocation (2) (7.51) 0 has Burgers vector b 1 , then the preceding analysis becomes: 0 σxx T b σ = b|010| σyx % &' ( 0 (2) %

σxy 0 σyy 0 = b|σxy σyy 0| , 0 σzz &' (

(7.52)

(1)

i j k f = bT σ × s = b σxy σyy 0 = bσyy i − bσxy j . (2) 0 0 1

(7.53)

In this case, the x-component of the force produces a positive climb force to the right, and the y-component of the force produces a negative (downward) glide force. Screw–screw interaction For two screw dislocations as shown in Fig. 7.34, the force on dislocation (2) due to dislocation (1) is: i j k (7.54) f = bT σ × s = b σxz σyz 0 = bσyz i − bσxz j , (2) 0 0 1 where the x-component of the force, bσyz is to the right, and the y-component of the force, −bσxz is downward in Fig. 7.34. The force on dislocation (2) can be written as: F=

μ bb(2) cos θ i + sin θ j , 2π r

(7.55)

and the force components in the x–y plane have already been shown in Fig. 7.30a, and as a function of θ in Fig. 7.30b.

Fig. 7.34. Orientation of dislocations to determine the force on screw dislocation (2) due to screw dislocation (1)

292

7 Dislocation Microstructure Fig. 7.35. Orientation of dislocations to determine the force on screw dislocation (2) due to edge dislocation (1)

Edge–screw interaction The last example is the determination of the force between an edge and a screw dislocation as defined in Fig. 7.35. We know that an edge dislocation has no xz or yz stress components, which are needed to move a screw So we can state dislocation. 0 1 the following rules: For an edge dislocation with b 0 and s 0 , the only stresses 1 0 that produce a force on it are σxx and σxy . The stress field around thedislocation has 0 0 components σxx , σyy , σzz and σxy . For a screw dislocation with b 0 and s 0 , the 1 1 only stresses that produce a force on it are σxz and σyz . The stress field around the dislocation has components σxz and σyz . 7.1.8 Extended Dislocations Slip occurs in the fcc lattice on (111) planes and in the 110 direction. The Burgers vector is a/2[110], which is the shortest lattice vector connecting an atom at the cube corner with a neighboring atom at the center of a cube face. However, the atom arrangement on the {111} slip plane is such that slip in the [110] direction is not the easiest path. Figure 7.36a shows the atom arrangement on a close-packed (111) plane. The {111} planes are stacked in the sequence ABC ABC. . . ., such that the centers of the A plane of atoms fall on top of each other, ¯ shown and similarly for the B and C planes of atoms. The vector b1 = a/2[101] in Fig. 7.36a is the observed slip direction. However, if atoms are considered as hard spheres, this direction represents a high-energy path as atoms moving from one B site to another must climb over the A atoms. A simpler path is by way of vectors b2 and b3 , which is along the “valleys” between the A atoms. This dislo¯ → a/6[21¯ 1] ¯ + a/6[112]. ¯ Essencation reaction is given by: b1 → b2 + b3 , a/2[101] tially, the Burgers vector, b1 of the total dislocation has been dissociated into two partial dislocations b2 and b3 . Figure 7.36b shows the atom arrangement of the partial dislocations on the {111} plane and Fig. 7.36c shows the vector diagram

7.1 Dislocation Lines

293

Fig. 7.36. Slip on the close-packed (111) plane in the fcc lattice. (a) Slip directions. (b) Location of atoms in a Shockley partial. (c) Dislocation dissociation into to partial dislocations

of the dissociation of the total dislocation into two partial dislocations. The partials are often called Shockley partials and the combination of the two partials is termed an extended dislocation. Dissociation is independent of dislocation character and the partial dislocations move as a unit that maintains the equilibrium width between them. The space between the partials is referred to as the faulted region or the stacking fault and its size is determined by the stacking fault energy, SFE. The lower the SFE, the greater the separation of the partials and the higher the energy, the closer they are together. Stacking faults are important in cross slip as the partials must recombine in order for cross slip to occur. Ex-

294

7 Dislocation Microstructure

tended dislocations also occur in hcp lattices, but are not commonly observed in bcc metals. 7.1.9 Kinks and Jogs Both edge and screw dislocations can acquire jogs, or steps in the dislocation line by interaction with other dislocations. The jogs are of two types. A jog that lies in the slip plane instead of normal to it is called a kink. Figure 7.37a shows an edge dislocation with a kink of screw character that lies in the slip plane of the edge dislocation, and Fig. 7.37b shows a screw dislocation with a kink of edge orientation. Kinks are unstable as they can line up and annihilate during glide. A second type of jog is shown in Fig. 7.37c in which the jog and the dislocation are of edge orientation. These types of jogs are able to glide since they lie in the slip plane of the dislocation. The only difference between the motion of the jogged edge dislocation and the ordinary edge dislocation is that instead of gliding along a single plane, it glides over a stepped surface. Another type of jog is the most important in plastic deformation and is shown in Fig. 7.37d. This is a screw dislocation containing a job with an edge orientation. The only way the screw dislocation can move to a new position and take its jog with it is by climb of the jog. Figure 7.37e shows the movement of a jogged screw dislocation as the segments between jogs bow out in the slip plane under an applied stress producing a trail of vacancies left behind the jog as the dislocation moves in its slip plane.

7.2 Faulted Loops and Stacking Fault Tetrahedra Because of their importance in irradiated materials, we will discuss Frank loops at greater length. Frank loops are important in irradiated materials because they are often nucleated in a displacement cascade. Recall that the cascade consists of a core of vacancies surrounded by a shell of interstitials (Figs. 3.3 and 3.9). If the vacancy core or the interstitial shell collapse (condense) onto a close-packed plane, Frank loops may be generated. In both cases, a stacking fault results. Vacancy condensation produces an intrinsic fault and interstitial condensation results in an extrinsic stacking fault. The faults are described as follows. In regular, close-packed lattices such as fcc and bcc, atom layers follow a regular stacking sequence. In the fcc lattice, the stacking sequence is ABCABCABC. . . , indicating that every third layer lies over the first layer. Removal of a layer of atoms results in a break or a fault in the stacking sequence. Removal of a plane of atoms produces an intrinsic stacking fault, which is also known as a single fault, and the dislocations attached to the single fault are S-dislocations, giving an S-Frank dislocation (Fig. 7.38a). For example, the sequence is modified to ABCAB/ABCABC. . . , where “/” denotes the fault or missing plane of atoms. Insertion of an extra plane of atoms produces a double fault in the stacking sequence; ABCAB/A/CABC. . . . (Fig. 7.38b). This is an extrinsic or double fault and the dislocations are D-dislocations giving a D-Frank loop. The Burgers vector of the S-Frank

7.2 Faulted Loops and Stacking Fault Tetrahedra

295

Fig. 7.37. Kinks and jogs in dislocations. (a) Edge dislocation with a kink of screw character. (b) Screw dislocation with a kink of edge orientation. (c) Edge jog in an edge dislocation. (d) Edge jog in a screw dislocation and direction of motion of the dislocation. (e) Movement of a jogged screw dislocation of part (d) showing bowing of the segments between jogs and the trail of vacancies left behind the trail of jogs (after [7])

296

7 Dislocation Microstructure

Fig. 7.38. Schematic of an (a) intrinsic stacking fault and an (b) extrinsic stacking fault

and D-Frank loops are identical. Since a Frank loop results from addition or removal of close-packed planes, b must be directed√normal to the (111) plane and has a length equal to the spacing between planes, a/ 3, then the Burgers vector is described by b = a/3[111]. Since it is extremely difficult to move on its slip plane (the glide plane is actually a cylinder defined by the edge of the loop), the Frank loop is considered to be sessile or immobile since its glide plane is a cylinder defined by the projection of the loop perimeter in a direction perpendicular to, and above or below the plane of the loop. A Frank loop can also unfault either autocatalytically or by reaction with a dislocation line to form a perfect loop. This process is described in Chap. 12. Another dislocation configuration that can form in irradiated metals is the stacking fault tetrahedron (SFT). A SFT is a three-dimensional stacking fault configuration that is in the shape of a tetrahedron. SFTs are believed to evolve directly from vacancy clusters produced in cascades. They are also believed to evolve from Frank loops. A Frank loop will always line on a (111) plane in an fcc lattice. Figure 7.39a shows a loop of triangular shape on a (111) plane with edges parallel to [110] directions. A Frank dislocation that is parallel to a [110] direction can lower its energy by splitting into a Shockley dislocation, a/6[211] and a stair-rod dislocation. The slip plane of the Shockley dislocation is also a (111) plane but it is different from that containing the Frank loop. Figure 7.39b shows two of the three Shockley dislocations formed from the three sides of the Frank loop, moving up (111) planes. Each Shockley has left behind it a stair-rod dislo-

7.2 Faulted Loops and Stacking Fault Tetrahedra

297

Fig. 7.39. A stacking fault tetrahedron (SFT) formed by faults on each of the faces of the tetrahedron (after [1])

cation, a/6[110] in the position formerly occupied by a side of the Frank dislocation loop (edge of the triangle). The stacking fault contained in the Frank loop now bends at the stair-rod dislocation and extends up onto the close-packed (111) planes of the Shockley dislocations. As the Shockley dislocations move up the planes shown in Fig. 7.39b, they eventually meet at the intersections of their slip planes and the intersections of Shockley dislocations result in other stair-rod dislocations along the remaining three edges of the tetrahedron. The final configuration is a tetrahedron whose sides are stacking faults and whose edges are stair-rod dislocations (Fig. 7.39c). The Frank dislocation and the Shockley dislocations no longer exist. Dislocations can also interact with SFTs. MD simulation of the interaction of a dissociated a/2[110] dislocation (into two Shockley partials, a/6[121]) on the (111) glide plane shows that several types of interaction are possible [8]. When the SFT is in the slip plane of the dislocation, the SFT may be cut by the dislocation

298

7 Dislocation Microstructure

and recovers by a shift of the structure above the glide plane to regain its original shape. The interaction can also create ledges in the SFT that can reduce stability and lead to dissolution. TEM observations show that SFTs can be cut multiple times by dislocations in channels.

7.3 Defect Clusters As described in Chap. 3, the fraction of defects produced in a cascade is between 20 and 40% of that predicted by the NRT model due to intracascade recombination. Of these, not all appear as single interstitial atoms or isolated vacancies. A significant fraction of defects are created in the form of clusters, rather than as single defects. Vacancy clusters may grow to form voids, which are an important microstructure feature that influences both dimensional (Chap. 8) and mechanical (Chap. 12) properties of materials. If the clusters are stable, they may also migrate away from the cascade region and be absorbed at sinks such as dislocations and grain boundaries. Interstitial and vacancy clusters must be treated separately since in general, interstitial clusters are stable and vacancy clusters are not. Their mobilities differ as well with interstitial clusters exhibiting greater mobility than their vacancy counterparts. 7.3.1 Fraction of Defects Forming Clusters In-cascade clustering of defects is important because it promotes nucleation of extended defects. Interstitial clustering can occur in one of two ways. In the first, interstitial clusters are created in the transition between the collisional and thermal spike phases in which atoms that are displaced from the cascade center due to the initial shock wave are pushed into interstitial locations. Alternatively, clusters can occur during the thermal spike phase by short-range diffusion driven by the elastic interaction between neighboring interstitials. The probability of clustering and the size of the clusters tend to increase with increasing PKA energy and a higher proportion of SIA form clusters than do vacancies [9]. Figure 7.40 shows the fraction of interstitials that form clusters as a function of the PKA energy in several metals and at 100 K, as determined by MD simulation [10]. Note that the clustered fraction increases quickly with T as damage transitions from single displacements to cascade morphology. In contrast to the Frenkel pair production efficiency (Fig. 3.20) the clustered fraction varies with the metal, and while there are only 5 metals shown here, the clustering appears to occur according to the crystal structure with the highest clustering fraction occurring for the fcc structure and the lowest for the bcc structure with the hcp structure in between. While MD results show that the fraction of interstitials in clusters is larger in copper than in α -iron by ∼ 70 to 45% at 100 and 600 K for PKA energies above 5 keV [11], experimental evidence shows that the cluster density in copper is as much as 103 higher than that in Fe [12]. While the size of this difference is not

7.3 Defect Clusters

299

Fig. 7.40. The fraction, ficl , of SIAs that survive as clusters containing at least two interstitials in several metals and Ni3 Al at 100 K (after [10])

understood, it may have its origins in the nature of the cluster as discussed in the next section. Interstitial clustering depends on the irradiation temperature [9, 10, 13]. Figure 7.41 shows that with increasing temperature, the fraction of interstitials in clusters in α -iron decreases for damage energies between 5 and 40 keV. Actually, interstitial clustering increases at higher temperatures due to the more compact nature and longer lifetime of the cascade at higher temperature, providing more time for interstitials to diffuse and interact. Recall from Sect. 3.6 and Fig. 3.21 that the Frenkel pair production decreases slightly with temperature. Combining these results, the effect of temperature can be described as resulting in an increasing fraction of the decreasing population of interstitials forming clusters as the temperature increases, yielding a net decrease in fid .

Fig. 7.41. The fraction of SIA clusters formed in a sessile configuration in α -iron at the end of the thermal spike as a function of PKA energy and irradiation temperature (after [10])

300

7 Dislocation Microstructure

Fig. 7.42. The fraction ficl , of SIAs that survive in clusters of two or more, three or more and four or more in copper at 100 K (after [10])

Finally, the clustered fraction can be broken down according to cluster size to reveal the dependence of clustering on cluster size. Figure 7.42 shows the fraction of SIAs in clusters of sizes 2, 3 and 4 in copper as a function of damage energy for an irradiation temperature of 100 K. Note that the cluster fraction is very sensitive to minimum cluster size, especially at lower damage energies, yielding a net decrease in ficl . Clustering of vacancies occurs within the core of the cascade as well and the extent of clustering varies with the host lattice. Based on measurements of size and number density of vacancy clusters in irradiated metals, the fraction of vacancies in clusters is estimated to be less than 15%. The true fraction may be larger because of the invisibility of small clusters, but also the fact that vacancy clusters are not nearly as stable as interstitial clusters as will be shown in the next section. 7.3.2 Types of Clusters The structure of the cluster is a strong function of the crystal structure [12, 14]. In α -Fe, MD simulation shows that the most stable configuration of small clusters (< 10 SIAs) is a set of 111 crowdions. Next in stability is the 110 crowdion. As the cluster size grows (> 7 SIAs) only two configurations are stable, the 111 and 110 crowdions. These crowdions also may act as nuclei for the formation of

7.3 Defect Clusters

301

Fig. 7.43. Binding energy for SIA loops of different shapes and Burgers vectors (a) in α -Fe, and (b) in copper (after [12])

perfect interstitial dislocation loops with Burgers vector 1/2111 or 100, respectively. In fcc copper, the 100 dumbbell is the stable configuration of the SIA and the smallest cluster is of the form of two 100 dumbbells. Larger clusters can have two configurations: a set of 100 dumbbells or a set of 110 crowdions, each with {111} as the habit plane. During growth, the clusters transform into faulted Frank loops with Burgers vector 1/3111, and perfect loops with Burgers vector 1/2110. The binding energy of SIA loops in Fe and in Cu is shown in Fig. 7.43a,b, respectively. Note that the binding energy for SIA loops in Cu is slightly higher than for SIA loops in α -Fe, in agreement with the higher clustering fraction predicted by MD modeling. Figure 7.44 shows a micrograph of interstitial clusters and small interstitial loops in a copper foil after irradiation with 30 keV Cu+ ions. Note that these defect clusters are only a few nanometers in size. Cluster densities can reach very high levels as shown in Fig. 7.45. The stability of vacancy clusters is low relative to interstitial clusters. The most stable configurations for vacancy clusters in α -Fe are either a set of di-vacancies concentrated on two adjacent {100} planes, or a set of first nearest neighbor vacancies on a {110} plane. During cluster growth, the first type results in a perfect dislocation loop with Burgers vector 100 and the second unfaults into a perfect

302

7 Dislocation Microstructure Fig. 7.44. Micrograph of interstitial clusters and small interstitial loops in copper irradiated with 30 keV Cu+ . Defects are highlighted by the circles on the micrographs (after [15])

Fig. 7.45. Dose dependence of cluster densities measured in α -iron and copper irradiated with fission neutrons at temperatures below 0.3 Tm (after [12])

7.3 Defect Clusters

303

Fig. 7.46. Binding energy of vacancy loops of different shapes and Burgers vectors in (a) α -Fe, and (b) copper (after [12])

loop with Burgers vector 1/2111. Vacancy loops can also exist in the faulted configuration. The loops will generally unfault to form perfect loops when the number of vacancies reaches about 40 [12]. In fcc Cu, the most stable configurations of a vacancy cluster are the stacking fault tetrahedron (SFT) and faulted clusters on {111} planes that form Frank loops with Burgers vector 1/3111. Binding energies of the various vacancy configurations in α -Fe and Cu are shown in Fig. 7.46a,b. Note that the binding energy of vacancies in the cluster is much less than that for interstitials shown in Fig. 7.43a,b. The binding energy per defect for a four-defect cluster is less than 0.4 eV for vacancies, but is about 1.2 eV for interstitials. Observation by transmission electron microscopy [16] reveals that vacancy dislocation loops and SFT a few nanometers in size are formed by cascades in many metals (Fig. 7.47).

304

7 Dislocation Microstructure Fig. 7.47. Transmission electron micrograph of (a) defect clusters in gold irradiated to 1.1 ×1022 n/m2 at 200 ◦C and (b) stacking fault tetrahedra in silver irradiated to 4.4 ×1021 n/m2 at 400 ◦C (after [16])

7.3.3 Cluster Mobility Clustered SIAs formed in cascades exhibit high mobility and can migrate over atomic scale distances during the lifetime of the cascade (∼ 10 ps). However, not all clusters are glissile. Besides stable, faulted Frank loops, SIAs may form metastable arrangement of SIAs that do not reorganize into a stable, glissile form by the end of the thermal spike. They are significant because they do not migrate away from the cascade, they may act as nucleation sites for the growth of extended defects. Figure 7.41 indicates that the fraction of SIA clusters in a metastable sessile configuration by the end of the thermal spike phase is between 30 and 50% at 100 K and somewhat less at 600 K. The form of these clusters varies with crystal structure. In hcp metals, small sessile clusters form a triangular arrangement of closely-packed atoms on the basal plane. In α -iron, three SIAs can form a triangle that is parallel to but displaced from the {111} plane. If clusters form as faulted dislocation loops, such as b = 1/3111 in fcc, 1/2110 in bcc and 1/20001 in hcp, then they are intrinsically sessile and cannot exhibit glide. The ability to move arises from the clustered crowdion form of these extended defects. They have a form best described as small perfect interstitial dislocation loops with Burgers vector b = 1/2110 in ¯ in hcp. Table 7.1 summarizes the fcc, 1/2111 and 100 in bcc and 1/31120 Burgers vectors of the glissile and sessile dislocation loops formed by vacancy and interstitial clusters. Mobile clusters can interact with other clusters or with impurity atoms such as helium. The behavior of small interstitial clusters in the presence of impurity helium atoms and vacancies is illustrated in Movies 7.1–7.3. In Movie 7.1 a SIA (green spheres) in bcc iron interacts with two substitutional He (light blue spheres) atoms and the interaction leads to recombination and ejection of the He into in an interstitial position from which it migrates and traps the other He substitutional atom. Movie 7.2 shows the interaction between a 6-SIA cluster and three substitutional He atoms. In this case, recombination and He ejection occurs with two of the three He atoms resulting in a cluster consisting of 4-SIA and one interstitial He atom, and

7.3 Defect Clusters

305

Table 7.1. Summary of Burgers vectors of glissile and sessile loops in fcc, bcc and hcp lattices (after [10]) Crystal structure

Burgers vector

Cluster mobility

fcc

b = 1/2110 b = 1/3111 SFT (vacancy) b = 1/2111, 100 b = 1/2110 ¯ b = 1/31120 ¯ b = 1/21010, 1/20001

Glissile Sessile Sessile Glissile Sessile Glissile Sessile

bcc hcp

a cluster consisting of one interstitial He and one substituional He. Movie 7.3 shows the interaction between a 6-SIA cluster and a 4-He/6-vacancy cluster. Vacancies are denoted by the red spheres. The interaction causes the recombination and rejection of He resulting in a 4-He/1-SIA cluster. The majority of SIA clusters are glissile. Di- and tri-interstitial clusters in both α -iron and copper undergo one-dimensional glide along the crowdion direction [12]. In these small clusters, the crowdion can rotate such that glide occurs in an equivalent direction. This rotation results in essentially three-dimensional motion. The rotation frequency is lower for tri-interstitials and increases with temperature for both defects. Larger clusters are essentially perfect dislocation loops with a Burgers vector along the crowdion axis, so that their movement can be considered as thermally-assisted glide in one-dimension. Figure 7.48 shows 19 and 91interstitial clusters in α -iron. Both loops extend over six (220) planes as shown in the figures at the right of each cluster. The motion of these clusters is one-dimensional and along 111. A feature of cluster motion is that the effective correlation factor is greater than unity, i.e., a cluster that has moved one step has a high probability of making the next step in the same direction. Movie 7.4 is an MD simulation of a 19-SIA cluster in bcc iron at 287 ◦C. The cluster exhibits one-dimensional motion in the direction of the Burgers vector. The activation energy for cluster motion is between 0.022 and 0.026 eV in α iron and between 0.024 and 0.030 eV in copper [12]. The activation energy is weakly dependent on the size of the cluster, allowing the cluster jump frequency to be expressed as:

νn = ν0 n−S exp(− Em /kT ) ,

(7.56)

where Em is the average effective activation energy, ν0 is the size-independent, pre-exponential factor, and the term n−S is the cluster size dependence, where a value of ∼ 0.65 for s describes the cluster size dependence of the pre-exponential factor for both α -iron and copper. Figure 7.49 shows the total pre-exponential factor as a function of cluster size. This dependence is likely due to enhanced focusing of the crowdion configuration for SIAs in a cluster, which results in increased probability of successive jumps.

306

7 Dislocation Microstructure

¯ and (b) [001] projections. Filled and open Fig. 7.48. A 19 and 91-interstitial cluster in (a) [111] circles represent the centers of mass of 111 crowdions and split dumbbells, respectively. (c) Additional (220) lattice planes occupied by the clusters (after [17])

Vacancy clusters that form perfect dislocation loops are also intrinsically glissile. MD simulation shows that the mobility of perfect vacancy loops with b = 1/2110 and 1/2111 in Cu and α -iron respectively, is only slightly lower than that of a cluster of the same number of interstitial crowdions [12]. The result is shown in Fig. 7.50 for a 37-defect cluster. As long as they are in the form of perfect loops, they are mobile. Vacancy clusters that do not collapse to a dislocation structure or that form a Frank loop or SFT are immobile.

7.4 Extended Defects As described in the previous sections, vacancies and interstitials can cluster to form other types of defects that will be important in defining the effect of irradiation on both physical and mechanical properties of the solid. In principle a cluster of point defects could be one-dimensional (a line), two-dimensional (a disc), or threedimensional (a void). Vacancies and interstitials that cluster in numbers greater than those discussed earlier will agglomerate into specific configurations in the crystal lattice. In particular they will take up the minimum energy configuration, which in

7.4 Extended Defects

307

Fig. 7.49. Size dependence of the pre-exponential factor in Eq. (7.56) in (a) α -Fe and (b) Cu (after [12])

Fig. 7.50. Jump frequency vs. reciprocal temperature for vacancy loops (squares and diamonds) and SIA loops (circles) in Fe at 375 ◦C (after [12])

308

7 Dislocation Microstructure

three dimensions is a void, and in two dimensions is a loop or platelet with a thickness of magnitude equal to one Burgers vector and lying between adjacent closepacked planes. It may be envisioned that following the radiation damage event, the core of the displacement spike collapses (or the vacancies condense) onto the {111} plane, forming a vacancy disc. The energy of the disc can be written as: Ed = 2π rd2 γ ,

(7.57)

where rd is the disc radius and γ is the surface energy of the metal. For a small number of vacancies, the aggregate form with the least energy is the spherical void. The energy of the spherical void of radius rV is: 2 EV = 4π rV γ.

(7.58)

If Ω is the atomic volume then the number of vacancies in the void is: nV =

3 4 π rV . 3 Ω

(7.59)

The energy of the void written in terms of the number of vacancies is: ES = 4 π

3nvΩ 4π

2/3

√ γ = (6nv Ω π )2/3 γ .

(7.60)

For a large number of vacancies, the planar loop is a more stable configuration and this will be discussed shortly. Another possible configuration of a cluster of vacancies is the stacking fault tetrahedron as described in Sect. 7.2. The energy of the stacking fault tetrahedron, or SFT, is given by [4, 18, 19]:

√ μ Lb2 4L (7.61) ESFT = ln + 1.017 + 0.97ν + 3L2 γSFE , 6π (1 − ν ) a where ν is Poisson’s ratio, a is the lattice parameter, γSFE is the energy of the stacking fault and L is the length of the edge of the tetrahedron and L = a(n/3)1/2. A similar process involving interstitial condensation may occur around the edges of the depleted zone where high interstitial concentrations may exist. The condensation of interstitials onto a close-packed plane produces an extra layer of atoms and two breaks in the stacking sequence, as described in Sect. 7.2 For a disc of radius rL , the energy of a faulted loop (vacancy or interstitial) is: EL = 2π rLΓ + π rL2 γSFE ,

(7.62)

where the first term is the energy of the dislocation line and the second term is the energy associated with the stacking fault, and Γ is the energy per unit length of dislocation line. In the fcc lattice, faulted loops lie on the {111} planes, which have

7.4 Extended Defects

309

√ √ an atom density of 4/ 3a2 , or an area per atom of 3a2 /4. So the radius of a loop consisting of n vacancies (or interstitials) is: √ 1/2 3a2 n . rL = 4π

(7.63)

Approximating Γ with μ b2 , Eq. (7.32b) where μ is the shear modulus and b is the Burgers vector, Eq. (7.62) becomes: √ EL = 2 π μ b

2

3a2 n 4π

1/2

√ 3a2 n +π γSFE . 4π

(7.64)

More precise expressions for the energy of faulted and perfect loops are given in [4, 6, 18, 19, 20] and from [20], the energy of the faulted Frank loop is:

2 1 4rL μ b2 rL ln − 2 + π rL2 γSFE . (7.65) EF = 3 (1 − ν ) rc The energy of a perfect loop [16] is:

4rL 1 2−ν 2 1 + μ b2 rL ln −2 , EP = 3 (1 − ν ) 3 2(1 − ν ) rc

(7.66)

where rc is the dislocation core radius. Equations (7.65) and (7.66) refer to both interstitial and vacancy loops and from these equations, the difference in energy between a perfect loop and a Frank loop is:

2−ν 1 4rL 2 2 ΔE = π rL γSFE − μ b rL ln −2 . (7.67) 3 2(1 − ν ) rc Therefore, unfaulting is favorable if:

2−ν μ b2 4rL γSFE > −2 . ln 3π rL 2(1 − ν ) rc

(7.68)

Equations for a disc, void, perfect loop, faulted loop and SFT are plotted in Fig. 7.51a,b for 316 stainless steel and zirconium respectively. The values of the materials parameters are provided in the caption. Note that in general, faulted defects are more stable in zirconium than in stainless steel and voids are more stable in stainless steel than in zirconium. In stainless steel, voids are stable to relatively large sizes and the energy of the faulted loop remains below that of the perfect loop to large defect sizes. In zirconium, faulted loops and SFTs are more stable than voids. The high susceptibility to void swelling in stainless steel and the absence of voids in zirconium are in qualitative agreement with the formation energies for these extended defects according to Fig. 7.51.

310

7 Dislocation Microstructure

Fig. 7.51. Formation energy for various vacancy cluster defects in (a) 316 stainless steel, and (b) zirconium as a function of the log of the number of vacancies in the cluster. Material parameters for stainless steel are γSFE = 35 mJ/m2 , γ = 1.75 J/m2 , μ = 82 GPa. Material parameters for zirconium are γSFE = 102 mJ/m2 , γ = 1.40 J/m2 , μ = 33 GPa

7.5 Effective Defect Production

311

Since we have just shown that the void is a stable configuration only for small numbers of vacancies, how then can we observe large voids with the number of vacancies exceeding several orders of magnitude? It is well-established that for most metals, irradiation at low temperatures (< 0.2T /Tm ) results in aggregation of vacancies and interstitials to form clusters that are bound by dislocations, i.e., loops and stacking fault tetrahedra (in metals with low SFE). At higher temperatures, vacancies can also aggregate to form voids. Voids appear in a band of temperatures ranging from about 1/3 < T /Tm < 1/2 where insoluble gases such as helium have a strong effect on stabilizing voids. At temperatures less than 1/3T /Tm , vacancies are not mobile enough to reach the voids before annihilation with migrating interstitials. Also, loops formed by vacancy collapse of cascades are stable against thermal dissociation at low temperatures and hence, reduce the number of vacancies available for void growth. At very high temperature, the thermal equilibrium vacancy concentration becomes comparable with the radiation-induced vacancy concentration and voids tend to shrink by vacancy emission. The subject of void and bubble nucleation and growth will be discussed in more detail in Chap. 8.

7.5 Effective Defect Production With a better understanding of the importance of defect clusters, we can expand and refine our description of defect production. Microstructure evolution is ultimately controlled by the migrating defect fractions of vacancies and interstitials, MDFv,i . The most straightforward component of the MDF is the isolated point defect fraction, IDFv,i (discussed in Chap. 3), which is produced directly in the displacement cascade. A second component is the mobile cluster fraction, MCFi,v (discussed in Sect. 7.3.3) and is composed of mobile interstitial defect clusters and mobile vacancy clusters. The third component is defects released from clusters by evaporation, EDFv,i , and is most important for vacancies, and interstitials at very high temperatures. Taken together, these three sources of isolated defects comprise the migrating defect fraction, MDFv,i . Zinkle and Singh [21] constructed a flow chart to show the evolution of the various defect forms (Fig. 7.52), which is an expansion of the more simplistic case shown in Fig. 3.16 by inclusion of the processes in dashed boxes. Zinkle and Singh summarized experiments from which values for MDFv,i could be determined, and found that in general, 3% < MDFi < 10%, and 1% < MDFv < 10% where the percentages refer to the calculated NRT production rate. While there is considerable uncertainly regarding the quantitative values deduced from experiments, the range can be used to bound the expected available defect fraction. The significance of these processes is that they are not often addressed in traditional rate theory models of microstructure evolution. To create an accurate physical model of defect production and accumulation under cascade damage conditions, the following must be included:

312

7 Dislocation Microstructure

Fig. 7.52. Flow chart giving the contributions to the migrating defect fraction from isolated defects, mobile defect clusters and evaporating defects (after [19])

1. The production of a large fraction of defects heterogeneously in the form of vacancy and interstitial clusters with the remainder as isolated vacancies and interstitials 2. The bias for absorption of mobile interstitial clusters and freely migrating interstitials at sinks 3. The fractions of interstitials and vacancies in clustered or isolated forms that are not necessarily equal, which is equivalent to an asymmetric production of freely migrating fractions of vacancies and interstitials

7.6 Nucleation and Growth of Dislocation Loops

313

4. Vacancy evaporation from clusters formed during the cascade quench that results in a temperature-dependent contribution to the fraction of freely migrating vacancies As will be shown in subsequent sections and in the discussion of void formation and growth in Chap. 8, intracascade clustering and the thermal stability of interstitial and vacancy clusters cause an asymmetry in the supply of migrating vacancies and interstitials, termed the production bias and this bias represents a strong driving force for loop and void nucleation and growth.

7.6 Nucleation and Growth of Dislocation Loops Dislocation loops resulting from vacancy and interstitial condensation are created from clusters of the respective defects, and either shrink or grow depending on the flux of defects reaching the embryo. Once they have reached a critical size, the loops become stable and grow until they unfault by interaction with other loops or with the network dislocation density. The following sections describe the processes of loop nucleation, growth and unfaulting that determine the dislocation microstructure of a metal under irradiation. 7.6.1 Loop Nucleation Various attempts have been made to determine the nucleation rate of dislocation loops and voids. We will follow a treatment that is based on steady sate concentrations of vacancies and interstitials and assumes dilute solution thermodynamics, as develop by Russell et al. [22]. In this treatment, the effects of cascades are ignored. We will then introduce clustering theory and show how it can be applied to the loop nucleation problem to account for the formation of defect clusters in addition to point defects. We begin by expressing the nucleation rate of a defect cluster of size n as the flux of clusters between adjacent size classes in a phase space of cluster size. Considering only one type of defect (vacancies, for example), the flux between any two adjacent size classes can be written as: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) ,

(7.69)

Fig. 7.53. Illustration of the capture and emission processes governing the flux of clusters between adjacent size classes in a phase space of cluster size

314

7 Dislocation Microstructure

where ρ (n) and ρ (n + 1) are the number of n-mers (loops containing n vacancies) and (n + 1)-mers per unit volume. βv (n) is the rate of vacancy capture by a n-mer, and αv (n + 1)is the rate of vacancy loss by a (n + 1)-mer. The first term in Eq. (7.69) represents an addition to the n + 1 size class by capture of a vacancy by a void n-mer size class. The second term is a loss from the (n + 1)-mer size class by emission of a vacancy. Figure 7.53 shows the various processes described by Eq. (7.69) in phase space. At steady state, Jn = 0 and Eq. (7.69) becomes:

αv (n + 1) = βv (n)

ρ 0 (n)

ρ 0 (n + 1)

,

(7.70)

where ρ 0 (n) is the equilibrium concentration of n-mer vacancy loops. Substituting for αv (n + 1) from Eq. (7.69) into the expression for the nucleation rate, Eq. (7.70) yields:

ρ 0 (n) Jn = βv (n) ρ (n) − ρ (n + 1) 0 ρ (n + 1) (7.71)

ρ (n + 1) ρ (n) 0 − = −βv (n)ρ (n) 0 , ρ (n + 1) ρ 0 (n) 0 and the term in brackets is just the derivative of the ratio ρ (n)/ρ (n), or 0 ∂ ρ (n)/ρ (n) . The nucleation rate then becomes: ∂n ∂ ρ (n)/ρ 0(n) 0 Jn = −βv (n)ρ (n) , (7.72) ∂n where

ρ 0 (n) = N0 exp(−ΔG0n /kT ) ,

(7.73) per unit volume, and ΔG0n

is the free energy and N0 is the number of nucleation sites of forming the n-mer vacancy loop. The steady state nucleation rate of vacancy loops (consisting of k vacancies) can also be described as the product of the loop concentration, the jump frequency of the vacancy to the loop and the jump distance, and is given by: Jk = ρk0 βk Z ,

(7.74)

where ρk0 and βk are the values of ρ 0 (n) and βv (n) at the critical size, k, and Z is the Zeldovich factor that depends on the curvature of ΔG0n near the maximum, at the critical size. If ΔG0n is approximated by a parabola in this region (lower curve in Fig. 7.54), then:

Z= −

1 ∂ 2 ΔG0n 2π kT ∂ n2

1/2 ,

(7.75)

nk

where the derivative is evaluated at the critical loop size, nk . Its value is the width of ΔG0k at kT units below the maximum and is on the order of 0.05.

7.6 Nucleation and Growth of Dislocation Loops

315

Fig. 7.54. Schematic nucleation curves showing the various parameters which are important in cluster nucleation. ΔG0k is the activation barrier to nucleation if interstitials are not present, while ΔGk is the same quantity if interstitials are present during the vacancy cluster nucleation process (after [22]) Fig. 7.55. Illustration of the capture and emission processes governing the flux of clusters between adjacent size classes in a phase space of cluster size and including the effect of interstitial capture

Consider now the presence of interstitials in the vacancy loop nucleation formulation. The flux between any two size classes, say n and n + 1, now becomes: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) − βi(n + 1)ρ (n + 1) ,

(7.76)

where all terms are as previously defined, and βv (n + 1) is the rate of interstitial capture by a (n + 1)-mer. Interstitial emission is of low probability and is neglected. Figure 7.55 shows the various processes described by Eq. (7.76) in phase space. The rate of vacancy emission from a vacancy loop will be governed by temperature, size and lattice energetics. Since the defect fractions are as high as 10−4, a cluster has a defect in its immediate vicinity only this small fraction of time. The emission probability should be affected only slightly during this time interval and not at all otherwise. Therefore we conclude that αv is a value characteristic of a system without interstitials. Setting J = 0 in Eq. (7.76) is equivalent to equilibrating the size classes since there is no net flux between size classes. If we neglect interstitials, then from Eq. (7.76) we can write:

αv (n + 1) =

βv (n)ρ 0 (n) . ρ 0 (n + 1)

(7.77)

316

7 Dislocation Microstructure

Combining Eqs. (7.76) and (7.77) gives:

0 ρ (n) βi (n + 1) + Jn = βv (n) ρ (n) − ρ (n + 1) 0 . ρ (n + 1) βv (n) Since ρ 0 (n) = N0 exp(−ΔG0n /kT ), then we note that: 0 ρ 0 (n) δ Gn = exp , ρ 0 (n + 1) kT

(7.78)

(7.79)

where δ G0n ≡ ΔG0n+1 − ΔG0n . The term δ G0n is the difference between the free energies of creating loops of j + 1 and j vacancies from single vacancies at the prevailing supersaturation. We now define new functions of n, ρ (n) and δ Gn such that by analogy with Eq. (7.79):

ρ (n)

ρ (n + 1)

=

ρ 0 (n)

ρ 0 (n + 1)

+

βi (n + 1) = exp(δ Gn /kT ) , βi (n)

(7.80)

where

δ Gn = ΔGn+1 − ΔGn ,

(7.81)

βi (n + 1) in Eq. (7.81). βi (n) Using the expression in Eq. (7.81), we can re-write the equation for Jn in terms of ρ (n) by substituting Eqs. (7.80) into (7.78) to give: ρ (n + 1) ρ (n) Jn = βv (n) ρ (n) − ρ (n + 1) . (7.82) ρ (n + 1)

and ΔGn is not generally a free energy because of the term

Re-arranging Eq. (7.82) gives: Jn = −βv (n)ρ (n)

ρ (n + 1) ρ (n) − , ρ (n + 1) ρ (n)

and noting that:

ρ (n + 1) ρ (n) ρ (n) − ∂ ρ (n + 1) ρ (n) ρ (n) = , Δn ∂n

(7.83)

(7.84)

gives: Jn = −βv (n)ρ (n)

∂ [ρ (n)/ρ (n)] , ∂n

(7.85)

which is the basic flux equation. Re-arranging Eq. (7.85) by taking the natural log of both sides and summing from j = 0 to n − 1 gives: n−1 n−1 δ G0j ρ ( j) βi ( j + 1) , (7.86) ∑ ln ρ ( j + 1) = ∑ − ln βv ( j) + exp kT j=0 j=0

7.6 Nucleation and Growth of Dislocation Loops

and

ρ (n) ln ρ (0)

=

n−1

∑

j=0

317

δ G0j βi ( j + 1) − ln + exp . βv ( j) kT

(7.87)

We can identify two boundary conditions. The first is the quantity ρ (0), which may be evaluated by noting that as βi (n)/βv (n) → 0, ρ (0) = ρ 0 (0) and that ρ 0 (0) → N0 , is simply the number of nucleation sites per unit volume. Since N0 (and hence ρ (0)) is independent of void concentration, we can write: n−1 δ G0j −ΔGn ρ (n) βi ( j + 1) + exp , (7.88) = − ln ln = ∑ ρ (0) βv ( j) kT kT j=0 and ΔGn

δ G0j βi ( j + 1) + exp . = kT ∑ ln βv ( j) kT j=0 n−1

(7.89)

Since as βi (n)/βv (n) → 0, ρ (0) → ρ 0 (0) and ρ 0 (0) is just N0 , the number of nucleation sites per unit volume, we have then: −ΔGn ρ (n) = N0 exp , (7.90) kT and

ΔG0n = activation barrier without interstitials ΔGn = activation barrier with interstitials. The upper curve in Fig. 7.54 shows ΔGn as functions of n. Note that ΔGn is larger than ΔG0k , and requires a larger loop size due to the hindering effect of interstitials on the loop nucleation process. The maxima in the two curves occur at nk , ΔG0k and nk , ΔGk . Now, the steady state loop nucleation rate may be calculated from the expression for Jn in Eq. (7.85): Jk = Z βk ρk ,

(7.91)

which is the rate at which loops escape over the potential barrier of height ΔGk in units of loops/cm3 s. The term βk , is the rate of single vacancy impingement on a loop of size nk . The term Z is:

1/2 1 ∂ 2 ΔGn Z = − . (7.92) 2π kT ∂ n2 n k

The subscript indicates that the second derivative is to be evaluated at n = nk . As with Z in Eq. (7.75), its value is the width of Δ Gk at kT units below the maximum and is of the order of 0.05. The second derivative is found from Eq. (7.69) to be:

1 ∂ 2 ΔG0n 1 ∂ ΔG0 1 ∂ 2 ΔGn = , (7.93) exp kT ∂ n2 kT ∂ n2 kT ∂ n n n k

k

318

7 Dislocation Microstructure

giving:

ρk = N0 exp −ΔGk /kT ,

(7.94)

where ΔGk is determined by evaluating Eq. (7.89) at nk . The steady state nucleation rate will not be established immediately after a sudden change in supersaturation or temperature, but will lag by a characteristic time, τ , known as the incubation time and is given by [22]:

τ = 2(βk Z 2 )−1 .

(7.95)

Equations (7.89) and (7.94) also apply for interstitial loop nucleation except that Z , βk and ρk are for interstitial loops rather than for vacancy loops, and ΔGn for interstitial loops is: n−1 δ G0j βv ( j + 1) ΔGn = kT ∑ ln + exp , (7.96) βi ( j) kT j=0 where δ G0j is now the difference between the free energies of forming dislocation loops of j + 1 and of j interstitials (in the absence of vacancies), βk is the gross rate of interstitial capture by the loop of critical size and 1/Z is the width of ΔGn (for interstitials) a distance kT below the maximum at ΔGk , and the net number of interstitials in the critical nucleus is denoted by nk . The critical loop size, nk occurs at the maximum of ΔGn and is determined by solving ∂ ΔGn /∂ n = 0 for nk . More recent treatments of the nucleation rate call for setting the all the fluxes in Eq. (7.69) equal to the steady state flux, Jss , leading to a family of equations [23]: J1 = βv (1)ρ (1) − α (2)ρ (2) = Jss

(7.97)

J2 = βv (2)ρ (2) − α (3)ρ (3) = Jss J3 = βv (3)ρ (3) − α (4)ρ (4) = Jss .. . Jn−1 = βv (n − 1)ρ (n − 1) − α (n)ρ (n)

(7.98) (7.99)

(7.100)

k where n = nmax v . Letting the ratio of shrinkage to growth, αk /βv = rk for all k ≤ 2, and letting r1 = 1, the system of equations can be solved by multiplying the equations for Jk by the product of all the rk with k ≤ i. That is, Eq. (7.98) is multiplied by r2 , Eq. (7.99) is multiplied by both r2 and r3 , and so on. If the resulting set of equations is summed, all the rk are eliminated except r1 and rn to yield: n−1

βv (1)ρ (1) − α (n)ρ (n) ∏ r j J1 = Jss =

j=2

n−1 k

.

(7.101)

1 + ∑ ∏ rj k=2 j=2

The product term in the numerator is eliminated by noting that (1) for a nucleation problem, the concentration of the monodefect, ρ (1) will be much greater than ρ (n),

7.6 Nucleation and Growth of Dislocation Loops

319

and (2) the ratio of the shrinkage to growth terms r j is less than unity for n > n∗v . Therefore, Eq. (7.101) becomes:

n−1 k

Jss = βv (1)ρ (1) 1 + ∑

∏ rj

−1 .

(7.102)

k=2 j=2

The advantage of this method to compute Jss is the elimination of the Zeldovich factor and the approximations that must be made to compute it. Russell [22] determined that based on vacancy and interstitial parameters and their likely supersaturations in a solid under irradiation, that interstitial loop nucleation is easier than vacancy loop nucleation because interstitial loop nucleation is much less sensitive to vacancy involvement than is vacancy loop nucleation to interstitial involvement. The primary reason is that Si is expected to be several orders of magnitude greater than Sv during irradiation because of the very low equilibrium concentration of interstitials. Nevertheless, nucleation by this mechanism has been found to be difficult for both vacancy and interstitial loops, in contrast to the observation of stable loop growth after fairly low doses. 7.6.2 Clustering Theory The nucleation of loops is essentially a clustering process in which enough of one type of defect needs to cluster, in the presence of the other type of defect, to result in a critical size embryo that will survive and grow. The cluster will shrink or grow depending on the net condensation rate of defects on clusters. Generalizing the description of cluster behavior in phase space given in the last section, and taking a vacancy loop as an example, vacancy clusters, ν j consisting of j vacancies will shrink or grow according to: j ∞ dν j = K0 j − ∑ [βvn ( j) + βin ( j)]ν j − ∑ αvn ( j)ν j dt n−1 n=1 j−1

∞

n=1 ∞

n=1

+ ∑ βvn ( j − n)ν j−n + ∑ βin ( j − n)ν j+n

(7.103)

+ ∑ αvn ( j + n)ν j+n + additional loss terms n=1

where βvn and βin are the capture rates of migrating defect clusters νn or in by a cluster of size ν j , and αvn is the corresponding emission or thermal dissolution rate. The first term on the RHS is the direct production of clusters of size j. The second term is the loss of clusters from size class j due to absorption of a vacancy or an interstitial cluster of size n, where 1 n ∞. The third term is the loss of clusters from size class j due to emission of vacancy clusters of size n. The fourth and fifth terms are the addition of clusters to size class j due to absorption of vacancy clusters by smaller size classes, and the absorption of interstitial

320

7 Dislocation Microstructure

clusters by larger size classes. The sixth term is the addition of clusters to the size class j by loss of vacancy clusters from larger size classes and the “additional loss terms” allow for other mechanisms of contributing to the number of clusters in size class j. Equation (7.103) can be solved numerically without further simplification. But for large clusters and long irradiation times, the number of equations required would be extremely large. A major simplification is to require clusters to grow or shrink by only the addition or loss of single point defects, resulting in: dν j (t) = K0 j + β ( j − 1, j)ν j−1(t) + α ( j + 1, j)ν j+1 (t) dt − [β ( j, j + 1) + α ( j, j − 1)]ν j (t) , j ≥ 2 .

(7.104)

If it is assumed that j is a continuous variable and a Taylor series expansion is used in Eq. (7.104) to relate all functions to their values at size j, the simplified description is a continuum diffusional approximation in size space, known as a Fokker–Planck equation: * ∂ ν j (t) ∂ ) = K0 j (t) − ν j (t) [β ( j, j + 1) − α ( j, j − 1)] ∂t ∂j * 1 ∂2 ) ν j (t)[β ( j, j − 1) + α ( j, j + 1)] , + 2 2∂j

(7.105)

which is further simplified to:

∂ ν j (t) ∂ ∂2 = K0 j (t) − Fv j ν j (t) + 2 Dv j ν j (t) ∂t ∂j ∂j ∂ ∂ = K0 j (t) − Fv j ν j (t) − Dv j ν j (t) . ∂j ∂j

(7.106)

The first term on the RHS of Eq. (7.106) is the direct production rate of clusters of size j. The second term is the drift in size space driven by the excess condensation of one point defect type over another: Fv j = (zv DvCv − zi DiCi )

(7.107)

The drift term is responsible for the shift of the cluster size distribution to larger sizes. The drift term ensures that a large cluster will inevitably grow in a radiation field, but due to the evolving microstructure, the drift contribution is not constant with dose. Cluster evolution is also very sensitive to the ratio of the concentration of vacancies and interstitials, as Fv contains the difference in their contribution and can change sign. The result is that the sign of Fv depends on the overall microstructure. The third term is the diffusion in size space and Dv j is the irradiation-enhanced diffusion coefficient given by: Dv j = 1/2(zv DvCv + zi DiCi ) .

(7.108)

7.6 Nucleation and Growth of Dislocation Loops

321

Fig. 7.56. Development of the interstitial loop size distribution with dose in 316 stainless steel irradiated at a dose rate of 10−6 dpa/s and a temperature of 550 ◦C with ρd = 1013 m−2 (after [25])

The diffusion term causes the cluster size distribution to broaden with dose. The diffusion term accounts for the fact that two different clusters introduced at the same time at the same size may differ in size at a later time due to random encounters with point defects. Algorithms for the approximate solution of Eq. (7.106) are discussed by Golubov et al. [24]. The features of the Fokker–Planck equation are illustrated in Fig. 7.56 for the development of the interstitial loop size distribution for 316 stainless steel with initial dislocation density of 1013 m−2 , irradiated at 550 ◦C at a dose rate of 10−6 dpa/s. Note that with increasing dose, the mean loop size increases (drift term in Eq. (7.106)) and the size distribution broadens (diffusion term in Eq. (7.106)). As small clusters grow and their geometry changes, so does the capture efficiency for freely migrating defects. For very large cluster sizes, the Fokker– Planck equation is too simple as the defect production and cluster growth depend on the microstructure. The effect of the damage microstructure in the evolution of defect clusters must be accounted for in order to accurately predict their behavior. 7.6.3 Production Bias-Driven Cluster Nucleation As discussed both in Chap. 3 and in the Sects. 7.3 and 7.4 of this chapter, a significant fraction of point defects produced under cascade damage irradiation are in the form of mobile and immobile vacancy and interstitial clusters such that freely migrating interstitials and vacancies are produced in unequal numbers. This has led to the concept of production bias as a major driving force for microstructure evolution under cascade-producing irradiation, and is based on the premise that defects

322

7 Dislocation Microstructure

in clusters do not behave as freely migrating defects. In fact, as we have seen, interstitial clusters can be mobile and exhibit 1D and 3D glide. In some cases, the clusters remain mobile to very large size, though generally, there is a tendency toward the sessile state with increasing size. This picture of defect formation describes an asymmetry, or bias, in the production of freely migrating point defects under cascade damage conditions due to two sources: (1) the difference in the proportion of vacancies and interstitials that agglomerate into primary clusters, and (2) the difference in the thermal stability and mobility of the vacancy and interstitial clusters. Under cascade conditions, in addition to the probabilistic nature of point defect jumps, the random production, in space and time, of clusters also introduces fluctuations in the point defect fluxes to the sinks. The production bias model (PBM) is a framework for considering this added complication in the evolution of the microstructure under irradiation. Semenov and Woo [26] utilized the Fokker–Planck treatment of cluster dynamics presented in the last section to produce a revised description of the loop nucleation rate that incorporates the effect of small interstitial cluster generation in the collision cascade produced randomly in time and space. They considered that small, immobile interstitial clusters are continuously generated in collision cascades, and that these clusters can be treated as small dislocation loops. The probability density, P of an interstitial cluster with a size of n0 interstitials at a time t0 , to grow to a size of n interstitials at time t is: ∂ Pi (n,t) ∂ ∂ =− (7.109) Fi (n) − Di (n) Pi , ∂t ∂n ∂n where the diffusion term, Di (n) describes the spreading of the size distribution of interstitial loops in time due to random fluctuations in the isolated and clustered point defect fluxes and is given by: Di (n) = Dsi (n) + Dcl i (n) ,

(7.110)

with superscripts s and cl denoting single defects and clusters, respectively, and: π n 1/2 (zv DvCv + zi DiCi ) , (7.111) Dsi (n) = Ω b + 2, + 2 , N Nd K0 n 2 Ndv zv Dcl + z2i di2 . (7.112) i = 4b kv Nd2 ki Nd In the preceding, K0 is the effective point defect generation rate (cluster + 2and , free), Nd is the average number of point defects generated per cascade and Ndv,i is the 2 average of the square of the quantity, kv,i are the total sink strengths for vacancies and interstitials, zvi are the bias factors for vacancies and interstitials, and b is the magnitude of the Burgers vector. The drift term has two components, Fis (n), and Fic (n). Fis (n) =

2π ri (n) (zi DiCi − zv DvCv ) , Ω

(7.113)

7.6 Nucleation and Growth of Dislocation Loops

323

is the term that drives the growth rate of loops and the loop radius:ri = (ni Ω /π b)1/2 and Ci,v and Di,v are the average concentration and diffusion coefficient of the defects. 2π ri (n) n Fic (n) = x fil (x,t)W (x, n) dx , (7.114) Ω n0 is the rate of change in the loop size due to the absorption of smaller interstitial loops by coalescence. The function fil (n,t) is the distribution of interstitial loops which is related to the total loop number density, Nil (t) by: Nil (t) =

nmax nmin

fil (n,t) dn ,

(7.115)

and nmin is the size of the interstitial clusters at which they become mobile and nmax is the size at which they join the network. The term W (n , n) describes the coalescence between loops of sizes n and n (n < n): 1/2 2 (n)λd2 4ri (n ) 2 D (n) + D (n) + , (7.116) W (n , n) = λd 4 where λd is the mean free path between two consecutive coalescing events, is the climb velocity and D (n) is the climb diffusion coefficient due to the fluctuating point defect fluxes and is given as: D (n) = Ds (n) + Dcl (n) ,

(7.117)

with:

Ω (zv DvCv − zi DiCi ) , 4π b2ri (n) + , + 2 , 2 Nd K0 Ω cl 2 Ndv 2 Ndi D = + zi zv . 16π b2 kv Nd2 ki Nd2 Ds (n) =

(7.118) (7.119)

Subject to the boundary conditions: Pi (nmin ,t)|n0 ,t0 = Pi (nm ,t)|n0 ,t0 = 0 , the solution to Eq. (7.109) is given by Semenov and Woo [26] to be: n0 x Fis (x ) dx dx nmin exp − nmin Di (x ) Pm = , n0 Fis (x ) ∗) x dx exp −(1 − α dx nmin nmin Di (x )

(7.120)

(7.121)

where

α∗ =

Fic (n ) (nmin < n < n∗ < nm ) . Fis (n )

(7.122)

324

7 Dislocation Microstructure

The term α ∗ is the ratio of the rate of loop size change due to cluster coalescence to that due to point defect absorption, or essentially, the relative importance of cluster coalescence compared to defect absorption. Semenov writes the integrals in the exponential functions in Eq. (7.120) as:

s Fi (x) 2 fs 1/2 ds ds 1/2 dx = ln n +1 , (7.123) n − dcl dcl dcl n Di (x) where Fis (n) Dsi (n) Dcl i (n) , d = , d = . (7.124) s cl 1/2 1/2 n n n1/2 The two limiting cases are when defect absorption is unimportant, dcl → 0, and when cluster coalescence is minimal, ds → 0. For the case dcl → 0, Eq. (7.121) becomes: fs =

exp(− fs n0 /ds ) − exp(− fs nmin /ds ) exp(− fs nm (1 − α ∗)/ds ) − exp(− fs nmin (1 − α ∗)/ds ) × exp(α ∗ fs nmin /ds ) ,

Pm = (1 − α ∗)

(7.125)

and for the case ds → 0, Eq. (7.121) becomes:

1/2 1/2 1/2 1 + 2 fsn0 /dcl exp −2 fs n0 /dcl Pm = (1 − α ∗ )2 exp 2α ∗ fs nmin /dcl

. 1/2 1/2 − 1 + 2 fsnmin /dcl exp −2 fs nmin /dcl

- 1/2 1/2 / 1 + 2(1 − α ∗) fs nmin /dcl exp −2(1 − α ∗) fs nmin /dcl

. 1/2 1/2 . − 1 + 2(1 − α ∗) fs nmin /dcl exp −2(1 − α ∗) fs nmin /dcl (7.126) The behavior of Pm as a function of the number of interstitials in the cluster is shown in Fig. 7.57. In this case, α ∗ = 0 and the solid lines are for the case where ds → 0, Eq. (7.126), and the dashed lines are for the case were dcl → 0, Eq. (7.125). The dashed line at the lower left in the figure resulted when clusters are ignored. However, when clustering is considered (solid lines) the nucleation probability increases substantially. In fact, if we define εi0 to be the fraction of interstitials produced in cascades in the form of immobile clusters, and K0 is the interstitial production rate, then εi0 K0 /n0 is the production rate of interstitial clusters in the cascade, and the nucleation rate of interstitial loops is: J =

εi0 K0 Pm . Ω n0

(7.127)

Choosing the following values; εi0 = 0.4, Pm ∼ 10−6 , Ω ∼ 10−29 m3 , n0 ∼ 8, gives ∼ 5 ×1021 loops/m3 per NRT dpa. Given that loop densities are observed to be about this value, then the incubation dose is on the order of 1 NRT dpa. However, this value for the nucleation incubation time is high as small loops are readily observed in transmission electron microscopy of irradiated materials at fractions of a dpa.

7.7 Dislocation Loop Growth

325

Fig. 7.57. Interstitial cluster nucleation probability as a function of loop size. In this figure, α ∗ = 0 and the solid lines are for the case where ds → 0, Eq. (7.126), and the dashed lines are for the case were dc → 0, Eq. (7.125). The dashed line at the lower left in the figure is result when clusters are ignored (after [26])

7.7 Dislocation Loop Growth The growth of loops can also be determined from the Fokker–Planck equations that provide the size distribution of loops of all sizes (see Fig. 7.56). Applying Eq. (7.104) to the case of interstitial loops gives an equation of the form: di j = dt K0 j + [βv ( j + 1) + αi( j + 1)]i j+1 − [βv ( j) + βi ( j) + αi ( j)]i j + βi ( j − 1)i j−1 , (7.128) where i j is the concentration of interstitial loops of size j and the term on the LHS of Eq. (7.128) is the time rate of change of the population of interstitial loops of size j. The terms βk ( j) and αk ( j) are the absorption and emission rates of defects of type k from loops of size j. The first term on the RHS of the equality is the direct production rate of clusters of size j. Practically, this term is different from zero up to the tetrahedral cluster ( j = 4). The first term in square brackets is the production of clusters of size j by the emission of an interstitial or absorption of a vacancy by clusters of size j + 1. The second term in square brackets is the loss of clusters of size j by absorption of a vacancy or an interstitial, or emission of an intertstitial. The last term is the addition of clusters of size j by capture of an interstitials by clusters

326

7 Dislocation Microstructure

of size j − 1. Solution of Eq. (7.128) results in the loop size distribution as a function of time, which describes the evolution of interstitial loops with dose or time. Pokor et al. [27] used the Fokker–Planck formalism to model the evolution of a population of loops via chemical rate theory in a homogeneous medium. In their treatment, they allowed for production of clusters in the cascade containing up to four defects, and solved a set of equations for the concentration of defect clusters consisting of two equations for individual vacancies or interstitials and 2N equations for the population of loops up to size N. The physics of the formulation is contained in the expressions for the defect capture rates, β , and emission rates, α for each defect type, k as a function of the cluster size, given as [27]:

βk ( j) = 2π r( j)zc ( j)DkCk , Dk αk ( j) = 2π r( j)zc ( j) exp(−Ebk ( j)/kT ) , Ω

(7.129) (7.130)

where r( j) is the radius of an interstitial loop of size j, Dk andCk are the diffusion coefficient and concentration of defect k, zc ( j) is the bias factor for the interstitial loop of size j and Ebk ( j) is the binding energy of for a cluster of j defects of type k. Pokor [27] gives the following expressions for zc ( j) and Ebi : b 1 zli − zi , (7.131) zc ( j) = zi + a 8π a j li /2 Ebi = Efi +

Eb2i − Efi 0.8 ( j − ( j − 1)0.8) , 20.8 − 1

(7.132)

where zi is the bias factor for a straight dislocation line for interstitials, a is the lattice parameter and b is the Burgers vector, zli and ali are parameters used to describe the evolution of the bias with cluster size [28]. For the binding energy term, Efi is the formation energy of an interstitial point defect Eq. (4.16), Eb2i is the binding energy of a two-interstitial cluster and j is the number of defects in a cluster of size j and the expression comes from molecular dynamics simulations [29, 30]. In order to account for the effect of the annihilation of the network dislocation density with dose, they assumed that the rate of change of the density was proportional to ρ 3/2, giving dρ / dt = −Kb2ρ 3/2 , and resulting in a dislocation density that decreases as 1/t 2 (see next section). The network dislocation density in irradiated metals evolves toward a saturation value with increasing dose. In stainless steel, it has been observed to reach a saturation value of ∼ 6 ×10−10 cm−2 over a temperature range that spans 400 to 600 ◦C [31]. Cluster model results of the loop density and size for three grades of stainless steel irradiated at 330 ◦C and to doses up to 40 dpa calculated using Eqs. (7.128)–(7.132) are compared against measurements in Fig. 7.58 and show relatively good agreement. Dislocation recovery plays an important role in microstructure evolution as it represents a change in sink density. Failure to account for the recovery of the initial dislocation network would lead to a faster saturation of the loop structure in the 316 alloys. The most sensitive param-

7.7 Dislocation Loop Growth

327

Fig. 7.58. Evolution of the Frank loop (a) density and (b) size for 330 ◦C irradiation to high dose according to the cluster dynamics model of Pokor et al. (after [27])

eters controlling the irradiation microstructure are the temperature, dose, materials constants and the initial network dislocation density. Simpler treatments for determining the loop size distribution can be made by neglecting the formation of defect clusters larger than the tetra-interstitial, limiting the number of size classes and simplifying the cluster description. Stoller et al. [32] described the evolution of larger loops by the equation: di j −1 (7.133) = i j−1 τ −1 j − i j τ j+1 , dt where i j is the number of loops in a given size class with radius rL , and the τ j is the lifetime of a loop of size j against growth to the next larger size class: r j+1 drL −1 τj = drL , (7.134) dt rj

328

7 Dislocation Microstructure

Fig. 7.59. (a) Comparison of calculated maximum faulted loop density and low fluence fast reactor data as a function of temperature. (b) Dose dependence of faulted loop density for irradiation of solution annealed stainless steel at 500 ◦C (after [32])

and drL Ω = [ziL (rL )DiCi − zvL(rL )Dv (Cv − CvL )] , dt b

(7.135)

where ziL and zvL are given by Eq. (5.97) and CvL = Cv0 exp(EF Ω /kT ), where EF is the energy of a faulted loop from Eq. (7.65). Figure 7.59a shows a comparison of the temperature dependence of the calculated maximum faulted loop density and

7.8 Recovery

329

low fluence fast reactor data for 316 stainless steel with initial network dislocation densities of 3 ×1015 m−2 (solid line) and 3 ×1013 m−2 (dashed line). Figure 7.59b shows the dose dependence of the loop density for solution annealed 316 irradiated at 500 ◦C. Semenov and Woo [26] accounted for the effect of production bias by writing Eq. (7.135) for the rate of change in loop size to include terms due to interstitial cluster and vacancy cluster absorption:

Ω drL = [Ji − Jv + Jve + Jicl − Jvcl ] , dt b

(7.136)

where the Js are the fluxes due to single interstitials, single vacancies, vacancy thermal emission, interstitial clusters and vacancy clusters, respectively, and τd is the lifetime of the dislocation loop. Substituting for the fluxes [32] results in: 2 kV (εi − εv ) + kd2 z¯(1 − εi) K e K0 drL = − , (7.137) dt (ρN + ρL)b k2 K0 where K0 is the defect production rate, K e is the vacancy thermal emission rate, ρn and ρL are network and loop dislocation densities, εi,v are the fraction of interstitials and vacancies, respectively, that are immobilized by intracascade clustering, 2 are the sink strengths of voids and εv = εv − K e /K0 , zd is the dislocation bias, kV,d zd k2 dislocations, k2 is the total sink strength and z¯ = 2 c 2 . The steady state interstik + zd kd tial loop growth rate for 316 stainless steel with an effective point defect production rate of 10−7 dpa/s is shown as a function of temperature in Fig. 7.60. The growth rate is in units of Burgers vector, b per dpa. Note that the loop growth rate is low at low and high temperatures and peaks at an intermediate temperature of about 500 ◦C.

7.8 Recovery Growing dislocation loops eventually encounter either network dislocations or each other. The maximum radius to which a loop can grow, Rmax , is governed by the 4π loop density, ρL as given by ρL R3max = 1. When loops interact, they coalesce 3 and contribute to the network dislocation density. Interaction between individual dislocations and loops results in loop unfaulting that also contributes to the network (discussed in Chap. 12, Sect. 12.3). As the dislocation density increases, the rate of loop interaction with the network increases and the loop radius is further limited by the network dislocation density as described by Eq. (5.82), (π R2max )ρN = 1. However, observations of irradiated microstructures confirm that the dislocation density saturates, implying that there must also be a process for removal of network dislocations limiting their buildup. The process of recovery can explain the behavior of the dislocation density with irradiation. The rate of change of the dislocation

330

7 Dislocation Microstructure

Fig. 7.60. Interstitial loop growth rate in units of Burgers vector, b per dpa as a function of temperature for a 316 stainless steel (after [33])

density in a solid under stress at high temperature is assumed to behave according to:

ρ˙ = Bρ − Aρ 2 ,

(7.138)

where ρ is the density of mobile dislocations and A and B are constants. (Note that while the rate of dislocation density change given by Eq. (7.138) is phenomenological by nature, a more accurate description of the physical process is provided by Eq. (7.133)). The first term of Eq. (7.138) is the production rate of dislocations and the second term is the annihilation rate. The loss term is assumed to occur due to mutual annihilation of pairs of dislocations of opposite sign, which implies a reaction rate that is proportional to the square of the number of dislocations present at a given time. Garner and Wolfer [34] showed that the generation rate of dislocations is proportional to b2 φ ρ 1/2 , so that Eq. (7.138) can be written as:

ρ˙ = Bρ 1/2 − Aρ 3/2 ,

(7.139)

where B ∼ b2 φ and A ∼ c , where c is the climb velocity of the dislocation (see Chap. 14). At steady state ( dρ / dt = 0), and the saturation density is ρs = B/A. The solution to Eq. (7.138) is given as: " ρ (t) 1 − e−x + ρ0 /ρs (1 + e−x ) " = , (7.140) ρs 1 + e−x + ρ0 /ρs (1 − e−x )

7.8 Recovery

331

Fig. 7.61. (a) Calculated dislocation density evolution in 316SS at 500 ◦C using Eq. (7.139), for starting densities of 7 ×1011 cm−2 and 4 ×108 cm−2 , for cold-worked and annealed conditions, respectively (after [34]). (b) Measured dislocation density in 20% cold-worked and annealed 316SS after irradiation in EBR-II at 500 ◦C (after [35])

where ρ0 is the initial dislocation density and √ √ x = A ρs t = ρs c t .

(7.141)

Using a saturation density, ρs of 6 ×1010 cm−2 , and initial dislocation densities, ρ0 of 3 ×108 cm−2 for annealed 316 SS and 7 ×1011 cm−2 for 20% CW 316 SS, the dislocation densities calculated from Eq. (7.139) are shown in Fig. 7.61a. The relationship between x in Eq. (7.140) and fluence was defined by the case where

332

7 Dislocation Microstructure

the dislocation density for annealed 316 SS reached a value of 2 ×1010 cm−2 at 2 ×1022 n/cm2. Data are plotted in Fig. 7.61b. Note how well the model results of Fig. 7.61a agree with the data. This agreement also establishes that the original dislocations are no different from those produced during the irradiation with regard to their ability to absorb point defects.

7.9 Evolution of the Interstitial Loop Microstructure The evolution of the interstitial loop population can be described in terms of its response to temperature and dose. The temperature regime that is important for LWR operation is between 270 and 340 ◦C. Higher temperatures may be reached from gamma heating in certain thick components such as PWR baffle plates. This temperature range represents a transition region between what is commonly termed as low-temperature (50 – 300 ◦C) and high-temperature (300 – 700 ◦C) behavior. Below 300 ◦C, the dislocation microstructure is characterized by a high density of “black dots” (defect clusters that are too small to resolve in the TEM, < 2 nm), network dislocations and a low density of Frank loops. A very small percentage of the small loops in stainless steels are observed to be SFT, which is much less than the 25 – 50% of clusters in nickel or copper [10]. Near 300 ◦C, the radiationinduced microstructure changes from one dominated by small dislocation loops to one containing larger faulted loops and network dislocations (Fig. 7.62). Figure 7.63 shows large dislocation loops after irradiation at high temperatures. Above

Fig. 7.62. Effect of irradiation temperature in the range 50 – 400 ◦C on the components of the dislocation density in neutron-irradiated austenitic stainless steel (after [36])

7.9 Evolution of the Interstitial Loop Microstructure

333

Fig. 7.63. Images of large Frank loops in (a) a 300 series stainless steel irradiated at 500 ◦C to a dose of 10 dpa (from [37]), and (b-e) in irradiated aluminum, copper, nickel and iron, respectively (after [16])

334

7 Dislocation Microstructure

Fig. 7.64. Effect of temperature on the Frank loop density in the intermediate temperature region, 400 – 600 ◦C, for neutron-irradiated austenitic stainless steel (after [36])

300 ◦C, the Frank loop population begins to decrease. Figure 7.64 shows the sharp decrease in faulted loop density by a factor of over 1000 between 400 and 600 ◦C in neutron-irradiated austenitic stainless steels. The loop size increases with increasing temperature that eventually leads to an increase in the loop unfaulting rate which contributes to the reduction in Frank loop population at high temperature. Loop density increases rapidly to saturation at low irradiation temperatures. Figure 7.65 shows the increase in loop density in austenitic stainless steels irradiated near 300 ◦C. Loop size is relatively insensitive to fluence below about 300 ◦C. At these low temperatures, loop sizes and densities become dynamically stable as a population when a balance is reached between new loop formation and the destruction of existing loops. With increasing temperature in the low-temperature regime, the density of fine loops decreases and the loop size increases. The dislocation microstructure evolves into one composed of Frank loops and network dislocations above about 300 ◦C. Loop density saturates at a few dpa and the density is maintained (in a dynamic sense) at higher doses. The dislocation network density increases in proportion to the faulted loop density as temperature is increased though the overall dislocation density is expected to stay fairly constant between 300 and 370 ◦C. In the higher temperature regime (400 – 600 ◦C), the population consists of a low density of Frank loops and a dislocation network. Evolution may actually occur more slowly if other microstructural processes are also occurring such as void and bubble nucleation and growth.

Nomenclature

335

Fig. 7.65. Evolution of the Frank loop density and size in various austenitic stainless steels following irradiation to doses of up to 13 dpa at a temperature near 300 ◦C (after [38])

The description of defect cluster nucleation and evolution provides a backdrop for understanding the phenomenon of void growth discussed in the next chapter. As will be shown, void formation and growth is intimately linked to the production of defect clusters and their growth into loops, as these microstructures constitute critical sinks that will govern the fate of voids.

Nomenclature a A b Cv,i 0 Cv,i x d Dv,i Dk j Dl E Eb Ef El

Lattice constant Area of slip plane Burgers vector Concentration of vacancies, interstitials Thermal equilibrium concentration of vacancies, interstitials Strength of diffusive spread for clusters by the x process Diffusion coefficient of vacancies, interstitials Diffusion term in size space of defect k and cluster size j, Eq. (7.106) Climb diffusion coefficient Energy Binding energy Formation energy Dislocation loop energy

336

Em Em Fk j

7 Dislocation Microstructure

Pi (n,t) Pm r rc rL rk s T Sv,i ui j g vn V W zv,i Z

Migration energy Effective activation energy for cluster motion Drift velocity in size space of defect k and cluster size j Eq. (7.106) Effective Frenkel pair production rate of species j Change in free energy Standard free energy Cluster of n interstitials Boltzmann’s constant Total sink strength for vacancies, interstitials Length of dislocation line segment Length of edge of stacking fault tetrahedron Nucleation current. Also flux Defect production rate Vacancy thermal emission rate Stress exponent in relation between dislocation velocity and shear stress Unit vector Critical cluster size Average number of defects generated in a single cascade Number density of interstitial loop Number of lattice sites per unit volume. Also number of nucleation sites Probability of growing an interstitial cluster to size n in time t Loop nucleation probability Defect cluster radius Dislocation core radius Loop radius Critical cluster radius Positive direction of the dislocation line Temperature. Also PKA energy Supersaturation of vacancies, interstitials Components of the displacement vector Dislocation glide velocity Cluster of n vacancies Volume Work Vacancy, interstitial bias factor Zeldovich factor Eq. (7.75)

αj βj γ γSFE δ

Emission rate of species j Absorption rate of species j Shear strain,. Also surface energy Stacking fault energy Thickness of void shell

Gj ΔG G0 in k 2 kv,i l L J K0 Ke m n nk , nk Nd Nil N0

Nomenclature

εc εi j εi0 Γ λ λd μ ν ρ (n) νs Ω ρx σ , σi j σs σsD τ τd

Strain associated with the dislocation core Components of strain Fraction of interstitials produced in cascades in the form of immobile clusters Dislocation line tension Lam´e constant Mean free path between consecutive interstitial cluster coalescing events Shear modulus Poisson’s ratio. Also jump frequency Number density of defect clusters of size n Strength of drift term for clusters, by absorption of single defects Atomic volume Density of entity x Stress and components of stress Shear stress Value of shear stress that yields a dislocation velocity of 0.01 m/s Incubation time Eq. (7.95) Lifetime of dislocation loop

Subscripts c d i k L F N P

Dislocation core Dislocation Interstitial Critical cluster size Loop Frank loop Dislocation network Perfect loop

v 0

Vacancy Initial

Superscripts c cl s

Coalescence Clusters Single defects

Acronyms EDF IDF MCF MDF

Evaporating defect fraction Isolated point defect fraction Mobile cluster fraction Mobile defect fraction

337

338

7 Dislocation Microstructure

PBM PKA SFE SIA

Production bias model Primary knock-on atom Stacking fault energy Single interstitial atom

Problems 7.1 Draw billiard ball models of the extra half sheet of atoms which constitute the following dislocations: a) The a/2[110] edge dislocation in the (111) plane of the fcc lattice b) The a/2[111] edge dislocation on the (110) plane of the bcc lattice. 7.2 It is found experimentally that a certain material does not change in volume when subjected to an elastic state of stress. What is Poisson’s ratio for this material? 7.3 Determine the volume of a 10 cm diameter copper sphere that is subjected to a fluid pressure of 12 MPa. 7.4 Assuming that atoms are hard elastic spheres, show that Poisson’s ratio for a close-packed array of spheres is 1/3. 7.5 For a circular shaped disc lying on the (111) plane of an fcc crystal: a) Determine the energy as a function of the number of vacancies. b) How many vacancies could a spherical void have before it would spontaneously convert to a vacancy disc? 7.6 It is known that the amount of stored energy in a solid can be increased with the addition of dislocations. a) Calculate this energy for aluminum with a dislocation density of 108 cm−2 . b) It has also been suggested that this energy can be increased by application of a shear stress, σs . Given that the straight edge dislocations in part (a) are in the form of an equally spaced cubic shaped network, determine the shear stress, σs , needed to bow each dislocation segment into a half circle and calculate the increase in stored energy resulting. 7.7 Calculate the net density of edge dislocations in a thin simple cubic crystal with lattice parameter a = 2 ×10−8 cm if it is bent to have a radius of curvature of 10 cm. (The thickness of the crystal is no greater than 1 mm.) 7.8 In the circular shear loop shown in the figure below, let the x-axis be the direction of the Burgers vector shown in the drawing, the x-axis be in the plane of the loop but perpendicular to the direction of the Burgers vector, and the y-axis be perpendicular to the plane of the loop. Let θ be the polar angle of the circle measured from point A. At any point θ on the loop, the Burgers vector has an edge component be that is perpendicular to the dislocation line at that position and a screw component bs that is parallel to the line. a) Using the fact that the vector b with these components is constant (in magnitude and direction) at all points on the loop, derive expressions for be and bs as functions of θ .

Problems

339

b) Suppose a shear stress σxy is applied to the loop. Show that the resultant force on the dislocation line is always radially directed and has a magnitude σxy b.

7.9 Plot the stress fields surrounding an edge and screw dislocation as a function of θ . Specifically, plot the following: a) σxx , σyy and σxy vs. θ for an edge dislocation b) σxz and σyz vs. θ for a screw dislocation 7.10 For the dislocations in the figure below: a) Calculate the magnitude of the components of force on dislocation (2) due to dislocation (1). b) Repeat part (a) for angles of 0◦ , 30◦ , 45◦ and 90◦ . c) At θ = 30◦ , will dislocation (2) i) glide toward or away from dislocation (1)? ii) tend to climb up or down? Why?

340

7 Dislocation Microstructure

7.11 For the dislocations given in the sketch, find: a) The force on dislocation (2) due to dislocation (1) b) In which direction will dislocation (2) climb and/or glide? c) Describe the stress and temperature dependence of these two processes and under what circumstances each will contribute to creep.

(1) s = |001|, b = b|100| ¯ b = b|010| ¯ (2) s = |001|, 7.12 An edge dislocation having the properties s = k, and b = b j is on a plane x = X. Calculate the y-coordinates of the maxima and minima of the glide and climb forces (separately) that it would experience due to a fixed dislocation at the origin (s = k) for the following three cases: a) b = bi b) b = b j √ c) b = b(1/2i + 3/2 j). 7.13 An edge dislocation (1) with s = [001] and b = [100] is located a the origin of coordinate system. Another edge dislocation (2) with s = [001] and b = √a √ [ 2 2 0] is located a distance r away from (1) and 45◦ CCW from the xaxis. a) Calculate the glide and climb force on dislocation (2) due to dislocation (1). b) Make a graph of the force on dislocation (2) as a function of θ (for a given r) for 0 ≤ θ ≤ 2π . 7.14 Compute the local force on dislocation (2) due to dislocation (1) for the four examples of interaction between two perpendicular dislocations listed below: s1 = [001] ⎧ [100] ⎪ ⎪ ⎨ [100] b1 = [100] ⎪ ⎪ ⎩ [010]

s2 = [010] ⎧ [100] ⎪ ⎪ ⎨ [010] b2 = [001] ⎪ ⎪ ⎩ [010]

References

341

where the first dislocation passes through x = y = 0 and is parallel to the zaxis, and the second dislocation passes through x = X, z = 0 and is parallel to the y-axis. a) Show that the total force on dislocation (2) vanishes in all cases. b) If dislocation is able to flex, sketch the shape it is likely to assume, provided the fist dislocation passing through the origin remains straight.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23.

24. 25. 26. 27. 28. 29.

Weertman J, Weertman J (1964) Elementary Dislocation Theory. Macmillian, London Hull D, Bacon DJ (1984) Introduction to Dislocations. Pergamon, Oxford Friedel J (1964) Dislocations. Pergamon, New York Hirth JP, Lothe J (1982) Dislocations in Crystals, 2nd edn. Wiley Interscience, New York Reed-Hill RE, Abbaschian R (1994) Physical Metallurgy Principles, 4th edn. PWS, Boston Hull D, Bacon DJ (2001) Introduction to Dislocations, 4th edn. Butterworth Heinemann, Philadelphia Dieter GE (1976) Mechanical Metallurgy, 2nd edn. McGraw-Hill, New York, p 180 Osetsky YuN, Stoller RE, Matsukawa Y (2004) J Nucl Mater 329–333:1228–1232 Bacon DJ, Osetsky YuN, Stoller RE, Voskoboinikov RE (2003) J Nucl Mater 323:152– 162 Bacon DJ, Gao F, Osetsky YuN (2000) J Nucl Mater 276:1–12 Phythian WJ, Stoller RE, Foreman AJE, Calder AF, Bacon DJ (1995) J Nucl Mater 223:245–261 Osetsky YuN, Bacon DJ, Serra A, Singh BN, Golubov SI (2000) J Nucl Mater 276:65–77 Osetsky YuN, Bacon DJ, Singh BN, Wirth B (2002) J Nucl Mater 307–311:852–861 Stoller RE (2000) J Nucl Mater 276:22–32 Jenkins ML, Kirk MA (2001) Characterization of Radiation Damage by Transmission Electron Microscopy. Institute of Physics, Philadelphia, PA Kiritani M (1994) J Nucl Mater 216:200–264 Wirth BD, Odette GR, Marondas D, Lucas GE (2000) J Nucl Mater 276:33–40 Johnson RA (1967) Phil Mag 16(141):553 Jossang T, Hirth JP (1966) Phil Mag 13:657 Kelly BT (1966) Irradiation Damage to Solids. Pergamon, New York Zinkle SJ, Singh BN (1993) J Nucl Mater 199:173–191 Russell KC, Powell RW (1973) Acta Meta 21:187 Stoller RE, Odette GR (1987) In: Gerner FA, Packan NH, Kumar AS (eds) RadiationInduced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, pp 358–370 Golubov SI, Ovcharenko AM, Barashev AV, Singh BN (2001) Phil Mag A 81(3):643– 658 Ghoniem NM, Sharafat S (1980) J Nucl Mater 92:121–135 Semenov AA, Woo CH (2003) Phil Mag 813:3765–3782 Pokor C, Brecht Y, Dubuisson P, Massoud JP, Barbu A (2004) J Nucl Mater 326:19–29 Duparc AH, Moingeon C, Smetniansky-de-Grande N, Barbu A (2002) J Nucl Mater 302:143 Soneda N, Diaz de la Rubia T (1998) Phil Mag A 78(5):995

342

7 Dislocation Microstructure

30. Osetsky YN, Serra A, Victoria M, Golubov SI, Priego V (1999) Phil Mag A 79(9):2285 31. Garner FA, Kumar AS (1987) Radiation-Induced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, pp 289–314 32. Stoller RE, Odette GR (1987) In: Garner FA, Packan NH, Kumar AS (eds) RadiationInduced Changes in Microstructure: 13th International Symposium (Part I), ASTM STP 955. American Society for Testing and Materials, Philadelphia, PA, p 371 33. Eyre BL, Bullough R (1965) Phil Mag 12:31 34. Garner FA, Wolfer WG (1982) In: Brager HR, Perrin JS (eds) Effects of Radiation on Materials: 11th Conference, ASTM STP 782. American Society for Testing and Materials, West Conshohocken, PA, p 1073 35. Garner FA (1994) In: Frost BRT (ed) Materials Science and Technology, chap 6, vol 10A. VCH, New York, p 419 36. Zinkle SJ, Maziasz PJ, Stoller RE (1993) J Nucl Mater 206:266–286 37. Mansur LK (1994) J Nucl Mater 216:97–123 38. Edwards DJ, Simonen EP, Bruemmer SM (2003) J Nucl Mater 317:13–31

8 Irradiation-Induced Voids and Bubbles

The formation and growth of voids and bubbles is of intense interest for material performance in radiation environments at elevated temperature. The first observation of voids in irradiated metals was published by Cauthorne and Fulton in 1967 [1]. Voids can have a profound influence on material properties because solids undergo volumetric swelling when voids form and grow. It has been suggested that the US breeder reactor program experienced a setback of nearly a decade by this surprising observation, as scientists scrambled to understand this phenomenon and the consequences to reactor internals. Since that time, a great deal of effort has been expended toward understanding their formation and growth. Figure 8.1 shows examples of voids in irradiated stainless steel, aluminum and magnesium. Voids of this size and number density can cause tens of percent increases in volume, translating into significant changes in linear dimensions as well. The challenge of designing a reactor to accommodate swelling of this magnitude quickly becomes monumental. The formation and growth of voids shares much in common with bubbles. Yet because of their nature—a void is essentially an empty cavity—bubble mechanics are more complicated. It is by virtue of the fact that insoluble gases are formed by transmutation when certain metals are irradiated that drew attention to the subject of bubbles in irradiated metals. Under irradiation, it is possible for large numbers of inert gas bubbles to form, which significantly alter the physical and mechanical properties of metals. Fast and thermal spectrum reactors generate helium via transmutation, and the first wall of a fusion reactor is susceptible to bubble formation due to the high gas loading from reaction products in the plasma. Numerous examples exist in reactor systems where bubbles form and alter material properties, one of the most important being the structural materials of fission reactors. This chapter will address the theory of void and bubble nucleation and growth, along with elucidating the most important factors affecting these processes in reactor systems.

8.1 Void Nucleation The driving force for the formation of voids in solids is the supersaturation of vacancies due to irradiation defined by: Sv =

Cv , Cv0

(8.1)

344

8 Irradiation-Induced Voids and Bubbles

Fig. 8.1. Micrographs of irradiation-induced voids in (a) stainless steel, (b) aluminum (c) and (d) magnesium [2, 3]

where Cv0 is the thermal equilibrium concentration of vacancies. During irradiation, defects react to form clusters and the clusters either grow by absorption of defects of the same type, or shrink by absorption of defects of the opposite type. For a cluster of vacancies to grow into a void, there must be a net increase in the number of vacancies absorbed over the number of interstitials absorbed. Thus, we will be inter-

8.1 Void Nucleation

345

ested in the equilibrium void distribution function, ρ 0 (n) (where n is the number of vacancies in the void), which is developed by a supersaturation of vacancies in the solid. The distribution function gives the number of vacancy clusters in each size class. Under non-equilibrium conditions, there will be a net flux, J, of voids from one size class to the next larger size class. This is the nucleation current and is the quantity we are interested in finding. The presence of an inert gas in the nucleation process is then considered. 8.1.1 Equilibrium Void Size Distribution Analogous to the case of point defects (discussed in Chap. 4) and following the derivation in [4], the equilibrium void size distribution is determined from the change in Gibbs free energy of a system containing a distribution ρ 0 (n) of vacancy clusters: G = G0 + ∑ ρ 0 (n)Gn − kT ∑ ln wn , n

(8.2)

n

where G0 is the free energy of the perfect lattice, the second term is the work to form a void distribution, and the last term is the entropy contribution to the number of ways that the voids can be distributed in a lattice. The quantity Gn is the Gibbs free energy (reversible work) required to form a void of size n: Gn = Hn − T Sn = En + pn − T Sn ,

(8.3)

where En = the energy required to form a void of n vacancies n = volume change (= nΩ ) p = hydrostatic stress Sn = the excess entropy associated with the process wn = the number of ways of removing ρ 0 (n) voids of size n from the solid Neglecting the last two terms on the right, Gn reduces to Gn ∼ = En . For large values of n, the energy of the void can adequately be represented by the surface energy: EV = 4π R2V γ ,

(8.4)

where γ is the surface energy of the solid per unit area and RV is the void radius which is related to the number of vacancies in the void by: n=

4π R3V , 3Ω

(8.5)

where Ω is the atomic volume. The reader should note that the expression in Eq. (8.4) is the same as was developed in Eq. (7.58) and for the limiting case of a vacancy, Eq. (4.22). Equation (8.4) is, however, an approximation since the energy should properly include terms for the contraction of the surface and for the elastic energy stored in the solid (see Eq. (4.23)). Combining Eqs. (8.4) and (8.5)

346

8 Irradiation-Induced Voids and Bubbles

gives: En = (36πΩ 2 )1/3 γ n2/3 .

(8.6)

The last term in Eq. (8.2) is the product of the temperature and the mixing entropy. It can be obtained by calculating the number of ways in which voids can be distributed in a crystal containing N0 lattice sites per unit volume. The procedure is the same as that used for vacancies in Sect. 4.2 and results in: nρ (n) (N0 /n)! wn = . (N0 /n − ρ 0(n))!(ρ 0 (n))! 0

(8.7)

We now define the chemical potential of a void of size n as μn that is related to the Gibbs free energy by: ∂ G μn = . (8.8) 0 ∂ ρ(n) T,p,n

Substituting Eq. (8.7) into Eq. (8.2), using Stirling’s approximation for the factorial term in Eq. (8.7), and taking the derivative as required by Eq. (8.8) (∂ G = ∂ ΔG since ΔG = G − G0) gives:

0 ρ (n) μn = En + kT ln . (8.9) N0 We have neglected ρ 0 (n) compared to N0 because the void concentration is low. For monovacancies (n = 1), and Eq. (8.9) reduces to: Cv μv = Ev + kT ln . (8.10) N0 Since the equilibrium concentration of vacancies in a solid is given by: −Efv 0 Cv = N0 exp , kT substituting for N0 from Eq. (8.11) into Eq. (8.10) gives: Cv μv = kT ln = kT ln Sv . Cv0

(8.11)

(8.12)

The criterion for chemical equilibrium is that the chemical potential of reactants and products in the system be the same, i.e., n μv = μn .

(8.13)

Substituting Eqs. (8.9) and (8.12) into the criterion for chemical equilibrium, Eq. (8.13) gives:

ρ 0 (n) = N0 exp(n ln Sv − ξ n2/3) ,

(8.14)

8.1 Void Nucleation

347

where

ξ = (36πΩ 2)1/3

γ . kT

(8.15)

Substituting Eq. (8.15) into Eq. (8.14) and considering only the term inside the exponent, we have: n ln Sv − ξ n2/3 = n ln Sv −

(36πΩ 2 )1/3 γ n2/3 . kT

(8.16)

Expressing Eq. (8.14) as ρ 0 (n) = N0 exp(−ΔG0n /kT ) gives the following expression for ΔG0n : ΔG0n = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 ,

(8.17)

which is just the free energy change in the solid on forming a spherical void consisting of n vacancies on some particular site. A schematic of Eq. (8.17) is shown in Fig. 8.2 in which the free energy is plotted as a function of the number of vacancies in a void. Note that the first term decreases linearly with n while the second term increases as n2/3 . Accounting for the magnitude of the factors in each term, the resulting sum is a curve with a maximum at a value of n∗ . This is the critical size of a void embryo which must be achieved in order for the embryo to grow into a void. At the critical point, vacancy addition and removal both cause a reduction in

Fig. 8.2. Schematic illustration of ΔG0n , the free energy of formation of a spherical void consisting of n vacancies and the effect of thermal fluctuations on the critical size void embryo

348

8 Irradiation-Induced Voids and Bubbles

the Gibbs free energy of the system, so this is an unstable point. Above the critical size, addition of vacancies to the embryo causes a decrease in the free energy, which means that void growth is favored, while loss of vacancies causes an increase in the free energy, so this reaction is not favored. Note also that thermal fluctuations add an increment to the embryo size, pushing the critical size to a higher value, and thus making it more difficult to nucleate a stable void. 8.1.2 Void Nucleation Rate The nucleation rate of void embryos (consisting of n vacancies) can be described using the same formalism that was used to describe vacancy loop nucleation in Chap. 7 and developed in [5, 6, 7]. However, for the sake of continuity, that derivation will be repeated here for the case of void embryos. Recall from Eq. (7.74) that the nucleation rate of a void embryo of size n is given by: Jn = ρ 0 (n)βv (n)Z ,

(8.18)

where ρ 0 (n) is the concentration of voids of size n vacancies, βv (n) is the absorption rate and Z, the Zeldovich factor (defined in Sect. 7.6.1) and the void concentration is given by: −ΔG0n ρ 0 (n) = N0 exp , (8.19) kT where N0 is the number of sites on which voids can be formed, and ΔG0n is the change in free energy in the solid upon formation of the void and is given in Eq. (8.17). The value of ΔG0n for the critical void embryo size, ΔG0k (for embryo size nk ), is the activation barrier for void formation shown in Fig. 8.3 by the lower curve and is given as: 2/3

ΔG0k = −nk kT ln Sv + (36πΩ 2)1/3 γ nk

.

(8.20)

The void nucleation rate is the nucleation current given in Eq. (8.18). The void nucleation current, Jn , and activation barrier, ΔG0k , apply to the case where only vacancies are present. However, under irradiation, vacancies and interstitials are produced in equal numbers so the presence of interstitials must be accounted for. We now consider the case where interstitials can also impinge on voids. The analysis is similar to that just presented, but more complicated due to the introduction of another specie that will make void nucleation more difficult. Consider now, the nucleation of vacancy clusters on one particular kind of attractive site [4, 5, 6] such as the compressive stress field around a dislocation. The following assumptions are made: 1. The lattice is in thermal and dynamic equilibrium, which are minimally affected by displacement and thermal spikes. 2. Monovacancies and solvent monointerstitials are the only mobile point defects present.

8.1 Void Nucleation

349

Fig. 8.3. Schematic nucleation curves showing the various parameters which are important in void nucleation. ΔG0k is the activation barrier to nucleation if interstitials are not present, while ΔGk is the same quantity if interstitials are present during the nucleation process (after [6])

3. The defects obey dilute solution thermodynamics. 4. A steady state concentration of vacancies and interstitials exist. Assumption (1) is reasonable as thermal spike lifetimes are very short (10−12 s) and dynamical equilibrium should be attained in similar time intervals. Assumption (2) is generally not valid since gas atoms are often present and are known to play an important role in nucleation (treated in Sect. 8.1.3). Assumption (3) should be valid for low defect concentration (≤ 10−4 atomic fraction). The final assumption is a gross oversimplification since the microstructure continues to evolve with increasing dose causing sink strength, and therefore defect concentrations, to continually change. The following derivation of the void nucleation rate from kinetic considerations is similar to that for loops, in which the nucleation rate is expressed as the flux of clusters between adjacent size classes in a phase space of cluster size. A flux is the concentration times velocity or the product of concentration, jump frequency and jump distance. The flux between any two size classes, say n and n + 1, is: Jn = βv (n)ρ (n) − αv(n + 1)ρ (n + 1) − βi(n + 1)ρ (n + 1) ,

(8.21)

where ρ (n) and ρ (n + 1) are the number of n-mer (voids containing a net of n vacancies) and (n + 1)-mers per unit volume. βv (n) is the rate of vacancy capture by a n-mer, αv (n + 1) and βv (n + 1) are the rates of loss and interstitial capture by a (n + 1)-mer. The first term in Eq. (8.21) represents an addition to the n + 1 size class by capture of a vacancy by a void of n-mer size class. The second term is a loss from the (n + 1)-mer size class by loss of a vacancy, and the third term is a loss from the (n + 1)-mer size class by capture of an interstitial. Interstitial emission is of low

350

8 Irradiation-Induced Voids and Bubbles Fig. 8.4. Illustration of the processes governing the flux of between adjacent void sizes in a phase space of void size

probability and is neglected. Figure 8.4 shows the various processes described by Eq. (8.21) in phase space. Setting J = 0 in Eq. (8.21) is equivalent to equilibrating the size classes since there is no net flux between size classes (as we did in Sect. 7.6). If we neglect interstitials, then we can write Eq. (8.21) as:

αv (n + 1) =

βv (n)ρ 0 (n) . ρ 0 (n + 1)

(8.22)

Combining Eqs. (8.21) and (8.22) gives:

0 ρ (n) βi (n + 1) Jn = βv (n) ρ (n) − ρ (n + 1) 0 + . ρ (n + 1) βv (n) Since ρ 0 (n) = N0 exp(−ΔG0n /kT ), then we note that: 0 ρ 0 (n) δ Gn = exp , 0 ρ (n + 1) kT

(8.23)

(8.24)

where δ G0n ≡ ΔG0n+1 − ΔG0n . We now define new functions of n, ρ (n) and δ Gn such that by analogy with Eq. (8.24):

ρ (n)

ρ (n + 1)

=

ρ 0 (n)

ρ 0 (n + 1)

+

βi (n + 1) = exp(δ Gn /kT ) , βi (n)

(8.25)

where

δ Gn = ΔGn+1 − ΔGn ,

(8.26)

βi (n + 1) in Eq. (8.25). βi (n) Using the expression in Eq. (8.25), we can re-write the equation for Jn in terms of ρ (n) by substituting Eq. (8.25) into Eq. (8.23) to give: ρ (n + 1) ρ (n) Jn = βv (n) ρ (n) − ρ (n + 1) . (8.27) ρ (n + 1)

and Δ Gn is not generally a free energy because of the term

8.1 Void Nucleation

Re-arranging Eq. (8.27) gives:

ρ (n) ρ (n + 1) Jn = −βv (n)ρ (n) − , ρ (n) ρ (n + 1) and noting that:

ρ (n) ρ (n + 1) ρ (n) − ∂ ρ (n) ρ (n + 1) ρ (n) = , Δn ∂n

351

(8.28)

(8.29)

gives: Jn = −βv (n)ρ (n)

∂ [ρ (n)/ρ (n)] , ∂n

(8.30)

which is the basic flux equation. Re-arranging Eq. (8.25) by taking the natural log of both sides and summing from j = 0 to n − 1 gives: n−1 n−1 δ G0j ρ ( j) βi ( j + 1) , (8.31) ∑ ln ρ ( j + 1) = ∑ − ln βv( j) + exp kT j=0 j=0 and:

ρ (n) ln ρ (0)

=

n−1

∑

j=0

δ G0j βi ( j + 1) + exp . − ln βv ( j) kT

(8.32)

We can identify two boundary conditions. The first is the quantity ρ (0), which may be evaluated by noting that as βi (n)/βv (n) → 0, ρ (0) = ρ 0 (0) and that ρ 0 (0) → N0 , is simply the number of nucleation sites per unit volume. Since N0 (and hence ρ (0)) is independent of void concentration, we can write: n−1 δ G0j ρ (n) βi ( j + 1) ln + exp = ∑ − ln ρ (0) βv ( j) kT j=0 (8.33) −ΔGn = . kT Since as βi (n)/βv (n) → 0, ρ (0) → ρ 0 (0) and ρ 0 (0) is just N0 , the number of nucleation sites per unit volume, we have then: −ΔGn ρ (n) = N0 exp , (8.34) kT and

ΔG0n = activation barrier without interstitials, ΔGn = activation barrier with interstitials.

352

8 Irradiation-Induced Voids and Bubbles

The upper curve in Fig. 8.2 shows ΔGn as functions of n. Note that ΔGn is larger than ΔG0k , and requires a larger void size due to the hindering effect of interstitials on the void nucleation process. The maxima in the two curves occur at nk , ΔG0k and nk , ΔGk . Now, the steady state void nucleation rate may be calculated from the expression for Jn in Eq. (8.30): Jk = Z βk ρk ,

(8.35)

which isthe rate at which voids escape over the potential barrier of height ΔGk in units of voids/cm3 s . The term βk , is the rate of single vacancy impingement on a void of size nk . If clusters are assumed to be spherical, then the vacancy impingement rate is expressed by the rate constant for point-defect absorption by spherical sinks, Eq. (5.99). Since void embryos are small, the capture rate is of mixed-control type in which both diffusion and reaction rate limitations are of comparable magnitude:

βv (n) =

4π RV DvCv , 1 + a/RV

(8.36)

were a is the lattice parameter, and assuming that the rate at which vacancies leave a void depends on the size of the void but not on the concentration of vacancies or interstitials or details of the dynamics. Note that for large voids, a/RV → 0 and βv (n) has a pure diffusion character. The term Z , analogous to Z but in the presence of interstitials, is:

Z = −

1 ∂ 2 ΔGn 2π kT ∂ n2

1/2 nk

.

(8.37)

The subscript indicates that the second derivative is to be evaluated at n = nk . Its value is the width of ΔGk at kT units below the maximum and is on the order of 0.05. The second derivative is found from Eq. (8.25) to be:

1 ∂ ΔG0 1 ∂ 2 ΔG0n 1 ∂ 2 ΔGn exp = , (8.38) kT ∂ n2 kT ∂ n2 kT ∂ n n n k

k

giving: ρk = N0 exp −ΔGk /kT ,

(8.39)

where ΔGk is determined by evaluating Eq. (8.33) at nk . Since the critical void nucleus size is taken as the maximum of the ΔGn curve, differentiating Eq. (8.17) and substituting the result into Eq. (8.33) permits evaluation of ΔGn . The maximum in ΔGn is determined by setting ∂ ΔGn /∂ n = 0 and

8.1 Void Nucleation

353

solving for n: nk =

36πγ 3Ω 2

3 , β (n) − β (n + 1) v i 3(kT )3 ln βv0 (n)

where Cv /Cv,0 nk

= βv (n)/βv0 (n).

Since RV =

3 nΩ 4 π

(8.40)

1/3 , the radius corresponding to

is: rk =

kT ln

2γΩ . βv (n) − βi(n + 1) βv0 (n)

(8.41)

Note that as βi → βv , rk → ∞, which says that if the capture rate for vacancies and interstitials is the same, then the critical void embryo size would need to be ∞. Figure 8.5 plots ρ (n) as a function of cluster size n for various values of βi /βv for Sv = 430 and T = 623 ◦C. Note the effect of increasing the interstitial arrival rate for a fixed vacancy arrival rate. With increasing arrival rate ratio, (βi /βv ) the slope of the distribution, dρ / dn decreases everywhere. The reason is that increasing the interstitial flux increases the fraction of embryos of a given size n which actually shrink to the next smallest size (n − 1), whereas to maintain the constrained distribution requires that the increased fraction be balanced by a decreased concentration of nuclei of size n relative to that of size (n − 1).

Fig. 8.5. Concentration of void embryos as a function of their size when the net flow of embryos is constrained to be zero. The parameters are the arrival rate ratios βi /βv , and the nucleation rates (in s−1 cm−3 ) of the unconstrained system. For this example, T = 623 ◦C and Sv = 430. Solid circles indicate the minima of n(x) (from [8])

354

8 Irradiation-Induced Voids and Bubbles Fig. 8.6. Nucleation rate as a function of the vacancy supersaturation. The parameters are the arrival rate ratios, βi /βv and the temperature (after [8])

Increasing the arrival rate ratio also shifts the minimum in the distribution ρ (n) to larger sizes and to lower concentrations. Since the nucleation rate is proportional to ρ (n), it decreases tremendously by the deepening and widening of the minimum in ρ (n) as the arrival rate ratio increases. The nucleation rate in Fig 8.5 decreases about 6 orders of magnitude as the arrival rate ratio is increases from 0 to 0.97. To obtain void nucleation as βi /βv approaches 1 requires higher vacancy supersaturation. The strong dependence of nucleation on vacancy supersaturation is affected only very slightly by the arrival rate ratio. Figure 8.6 shows that a factor of 10 increase in supersaturation causes the nucleation rate to increase from 1 to 1015 nuclei/cm3/s at 627 ◦C. The effect of temperature on the vacancy concentration, C∗ required to give a fixed nucleation rate is shown in Fig. 8.7 by the set of curves identified by the arrival rate ratios, βi /βv . Over most of the temperature range, C∗ increases with increasing temperature even though the supersaturation Sv = Cv /Cv0 decreases. Note that Cv is high at low temperature where the diffusion coefficient is small and there is not much loss. Cv is small at intermediate temperature where annihilation and loss to sinks is great. But Cv is high again at high temperature where Cv0 ∼ Cv . The parameter p is the probability per defect jump that the defect is annihilated at a sink. The values of p range from 10−7, typical of an annealed metal to 10−3 , which is typical of a heavily cold worked metal.

8.1 Void Nucleation

355

Fig. 8.7. Steady state vacancy concentration caused by a production rate of K0 = 10−3 atom fraction of defect pairs per second. The parameter p on the curves is the probability per jump that a defect is annihilated at existing sinks, such as dislocations. The curve labeled Cv0 is the thermal equilibrium concentration of vacancies. The set of curves labeled by the arrival rate ratio, βi /βv indicates the vacancy concentration required to give a nucleation rate of 1012 void nuclei/cm3 s. This nucleation rate is obtained at the temperature and vacancy concentration at the intersection of the curves under the conditions characterized by the curve parameters. The nucleation rate will be higher (lower) at temperatures below (above) the intersection temperature at fixed values of the parameters (after [8])

Figure 8.8 gives the steady state vacancy concentrations for several defect production rates, K0 and several nucleation rates J and for a sink-annihilation probability of 10−7 and an arrival rate ratio of 0.99. The intersection of the defect production rate and the nucleation rate provides the vacancy concentration at the temperature of the intersection. Higher vacancy production rates promote greater vacancy concentration and a higher nucleation rate. In summary, the void nucleation rate is a function of the height of the activation barrier. Inclusion of interstitials raises the activation barrier and reduces the nucleation rate. The critical void size radius for survival and growth as a void is a function of the activation barrier height with greater heights requiring larger critical void sizes. Nucleation rate is strongly increased by vacancy supersaturation and a reduced interstitial-to-vacancy arrival rate ratio. 8.1.3 Effect of Inert Gas Up to this point, we have assumed that a supersaturation of vacancies was sufficient to create a void embryo. It is well-known that inert gas atoms may act to

356

8 Irradiation-Induced Voids and Bubbles

Fig. 8.8. Steady state vacancy concentrations for several defect production rates and a sink annihilation probability p = 10−7 , and vacancy concentrations required for several nucleation rates J (in cm−3 s−1 ) at an arrival rate ratio of 0.99. Such nucleation rates are obtained at the indicated defect production rates at the temperature where the curves intersect (after [8])

stabilize a void embryo and assist in the nucleation process. In fact, there is evidence to suggest that gas atoms are always involved in the void nucleation process [6, 7, 8, 9, 10]. Hence, several theories have been proposed that involve void nucleation in the presence of inert and non-inert gases [9, 11]. Here we will consider a simple treatment [4, 9] of an immobile, inert gas, which is just as extension of the theory already developed. We will focus on helium since it is commonly produced by transmutation reactions in core structural materials. Helium is very immobile compared to vacancies or interstitials in the temperature range of void formation. Once helium is trapped by a void embryo, its return to the matrix is very unlikely. Therefore, nucleation in the presence of helium does not require us to consider the interaction between helium atoms, vacancies and in-

8.1 Void Nucleation

357

Fig. 8.9. Phase space for void nucleation showing movements of a void following point defect capture (βi , βv , βx ) or loss (αv , αx , Kxc ) (after [6])

terstitials in the formation of a void embryo. We may analyze the problem instead, by treating the inert gas atoms as sites for the formation of void embryos by migration of the point defects. In essence, this is a form of heterogeneous void nucleation rather than the homogeneous process described in Sect. 8.1.2. The phase space description of the gas-containing void behavior is similar to that given in Sect. 8.1.2 and in [6]. The void is assigned coordinates specifying its vacancy content (n) and the number of gas atoms it contains (x) (Fig. 8.9). The void moves in the +n direction by capturing vacancies and in the opposite direction by either thermal emission of vacancies or capture of interstitials: n˙ = βv0 n1/3 − αv − βi0 n1/3 ,

(8.42)

where βv0 and βi0 are the arrival rates of vacancies and interstitials to the void, αv is the emission rate of vacancies from the void and the factor n1/3 accounts for the dependence of the capture rate on the void size. Similarly, movement in the positive x-direction occurs by gas atom capture and in the opposite direction by re-solution of gas atoms (return of the gas atom to the matrix due to knock-out by irradiation) or by thermal emission of gas atoms: x˙ = βx0 n1/3 − αx − xKxc ,

(8.43)

where βx0 is the arrival rate of gas atoms, αx is the emission rate of gas atoms and Kxc is the rate of gas atom re-solution. For the case where the voids are in equilibrium with the vacancy and gas atom concentrations, the distribution of gas-filled void embryos containing n vacancies and x gas atoms is:

ρ 0 (n, x) = N exp

−ΔG0 (n, x) kT

,

(8.44)

where ΔG0 (n, x) is the free energy of formation of the gas-filled void, also referred to as an (n, x)-mer. For every (n − 1, x)-mer capturing a vacancy, a (n, x)-mer will

358

8 Irradiation-Induced Voids and Bubbles

emit a vacancy, and for every (n, x − 1)-mer capturing a gas atom, a (n, x)-mer will emit one. Then:

ρ 0 (n − 1, x)βv0(n − 1)1/3 = ρ 0 (n, x)αv (n, x) ,

(8.45)

ρ 0 (n, x − 1)βx0(x − 1)1/3 = ρ 0 (n, x)αx (n, x) ,

(8.46)

and

and substituting Eqs. (8.45) and (8.46) into Eq. (8.42) to eliminate αv (n, x) and αx (n, x) gives:

βi0 1 ∂ ΔG0 (n, x) n˙ 1 − 0 − exp βv kT ∂n

c 1 ∂ ΔG0 (n, x) xKx 0 1/3 1 − 0 1/3 − exp , x˙ = βx n kT ∂x βx n = βv0 n1/3

(8.47) (8.48)

which are the velocities of the void in (n, x) phase space. However, we are interested in the nucleation rate, which requires more development and is described in detail in [4]. We start with a distribution of gas-atom clusters, Mx , which is the number of gas-atom clusters per unit volume composed of x gas atoms. The total helium concentration in the solid is: M=

∑ xMx ,

(8.49)

x=1

and is determined by the helium production rate due to transmutation reactions. We assume that nucleation of voids occurs independently and simultaneously on each of the gas atom clusters characterized by Mx nucleation sites per unit volume. Nucleation is driven by the vacancy and interstitial supersaturation. In addition to heterogeneous nucleation at gas cluster sites, homogenous nucleation is assumed to occur also on the N0 lattice sites in the solid. The total nucleation rate is the sum of the contributions of the homogeneous and heterogeneous nucleation rates: J = Jhom + ∑ Jx ,

(8.50)

x=1

where Jhom is given by Eq. (8.35). In order to obtain the total nucleation rate, we need to determine the heterogeneous nucleation rate Jx on the Mx gas cluster sites. The distribution of helium void embryos containing n vacancies and x gas atoms, ρ 0 (n, x) is governed by the reaction: nv = vnx ,

(8.51)

where vnx denotes a void consisting of n vacancies and x gas atoms. Since helium is immobile, there is no chemical reaction expressing the equilibration of gas atoms

8.1 Void Nucleation

359

between the voids and the bulk. The criterion of chemical equilibrium is then: n μv = μnx ,

(8.52)

and the chemical potential of a void with n vacancies and x gas atoms is:

μnx =

∂G . ∂ ρ 0 (n, x)

(8.53)

The formulation of the total Gibbs free energy for the gas-vacancy cluster is similar to the analysis presented earlier for vacancies alone. Analogous to Eq. (8.2) for voids, the total Gibbs free energy is: G = G0 + ∑ ∑ ρ 0 (n, x)Gnx − kT ln wnx . (8.54) x

n

As before, wnx is the number of ways of arranging ρ 0 (n, x) voids on Mi sites: ) * Mx (Mx − 1) . . . Mx − ρ 0 (n, x) − 1 Mx ! wnx = = . 0 0 [ρ (n, x)]! [Mx − ρ (n, x)]![ρ 0 (n, x)]! (8.55) Using Eq. (8.55) in Eq. (8.54) and using Eq. (8.54) to determine the chemical potential as given in Eq. (8.53) yields:

0 ρ (n, x) μnx = Gnx + kT ln . (8.56) Mx The reversible work to form a void embryo from n vacancies and x gas atoms is [4, 12]: MHnΩ Gnx = (36πΩ 2 )1/3 γ n2/3 − xkT ln . (8.57) xkT The first term is the work to create a gas-free void consisting of n vacancies, and is the same as that given in Eq. (8.6) for void formation. The second term is work to move the helium from the solid into the void. H in the second term is the Henry’s law constant for the dissolution of helium in the metal. The expressions for Gnx in Eq. (8.57) is substituted into the expression for the chemical potential of a void with n vacancies and x gas atoms, Eq. (8.56). Using the equality in Eq. (8.52) with μv given by Eq. (8.12) and solving for ρ 0 (n, x)gives:

MHnΩ 0 2/3 ρ (n, x) = Mx exp n ln Sv − ξ n + x ln . (8.58) xkT which is identical to Eq. (8.14) except for the extra term in the exponent and the preexponential factor. In fact, for x = 0 and Mx = N0 the result reduces to Eq. (8.14).

360

8 Irradiation-Induced Voids and Bubbles

Fig. 8.10. Plot of the free energy of void formation as a function of the number of vacancies (n) and the number of gas atoms (x) in the void. Conditions are: Sv = 600, p0 = 507 MPa, T = 500 ◦C, γ = 1 J/m2 (after [12])

Using Eq. (8.44) with Mx substituted for N0 gives: ΔG0 (n, x) = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 − xkT ln

MHnΩ xkT

.

(8.59)

Figure 8.10 shows the free energy of void formation as a function of n and x. The intercept of this surface at x = 0 (no gas) corresponds to the βi /βv = 0 curve in Fig. 8.5 in which ρ is plotted as a function of n in Eq. (8.34), ρ (n) = N0 exp(−ΔGk /kT ), and for βi /βv = 0, then ΔGn = ΔG(n, x = 0). Note that gas atoms in the void reduce the energy barrier for nucleation below that value characteristic of gas-free voids. The saddle point on the surface shown in Fig. 8.10 occurs at n = 11 and x = 6. The plot, however, does not include interstitials (as would a plot of ΔGn ), which are included in the analysis in exactly the same manner as in the case of homogeneous nucleation. The determination of the nucleation rate is done in the same manner as for homogeneous nucleation, resulting in a nucleation current: Jk,x = Zx βkx ρk (n, x) ,

(8.60)

8.1 Void Nucleation

361

Fig. 8.11. Void nucleation rates (J) on helium atom clusters and the homogeneous nucleation rate (Jhom ) as functions of vacancy supersaturation at 500 ◦C. Total helium content of 10 ppm (after [13])

where Zx =

−1 ∂ 2 ΔG (n, x) 2π kT ∂ n2

1/2 ,

(8.61)

ρ (n, x) = Mx exp(−ΔG (n, x)/kT ) ,

(8.62)

n=nk

and ΔG (n, x) = kT

0 βi 1 ∂ ΔG0 (n, x) ln + exp , ∑ βv0 kT ∂n x=0 n

(8.63)

and the values of zk and ρ (nk , x) are evaluated at the critical void size, nk , and βkx is the rate of impingement of vacancies on a critical size void. To determine the nucleation rate on the gas-atom clusters in the metal, we must estimate the distribution of the available gas (M atoms/cm3 ) among the various clus−(x+1) ter sizes. For simplicity, the distribution Mx = M1 is assumed. This distribution must satisfy Eq. (8.49). Figure 8.11 shows the results of calculations based on Eq. (8.60) to Eq. (8.62) and Eq. (8.60) for M equivalent to 10 ppm helium (equivalent to the amount of helium expected in stainless steel cladding after a fluence of 5 ×1022 n/cm2 ). Note that in the regime of vacancy supersaturation expected in a reactor, heterogeneous nucleation on helium-atom clusters far outweighs homogeneous nucleation. This behavior constitutes theoretical confirmation of the oftenobserved enhancement of void nucleation of helium. The relative importance of

362

8 Irradiation-Induced Voids and Bubbles

homogeneous and heterogeneous nucleation shifts according to the helium concentration because Jhom (n) is proportional to N0 whereas Jx (n) is proportional to Mx . At low fluence, homogeneous nucleation is dominant because there is not enough helium to drive heterogeneous nucleation. However, since Jhom is quite low, no voids are observed until sufficient helium has been generated by transmutation reactions to give the high heterogeneous nucleation rate. This incubation time is physically the relaxation time for the approach to steady state after a step increase in supersaturation. For void formation with or without the presence of gas:

τ = (2βk Z )−1 .

(8.64) 1022 n/cm2

This value is equivalent to a fluence of for fast reactor irradiation conditions. In summary, the effect of gas atoms is to substantially increase the void nucleation rate by lowering the critical radius for a stable void embryo below that for a gas-free void. Therefore, gas atom introduction into the lattice (either by transmutation or accelerator injection) promotes the formation of voids relative to the pristine lattice. 8.1.4 Void Nucleation with Production Bias The kinetic equation for dislocation loop evolution under cascade damage conditions was developed in Sect. 7.6.3 for interstitial clusters. We can use the same formulation with some changes to the terms to make the formulation specific to void nucleation [14]. Given that the number of vacancies in a spherical void can be written as: 1/3

dnv 3nv = 2 [DvCv − DiCi − DvCv0 ] dt a V 0 Cv = Cv exp(2γΩ /kT RV ) ,

(8.65) (8.66) 1/3

where a = (3Ω /4π )1/3, nv is the number of vacancies in a void, Rv = anv and Ω is the atomic volume, the drift velocity, F(n) (from the Fokker–Planck treatment) is now a single term equal to the RHS of Eq. (8.65). The diffusive spread, described by the term D(n) is a sum of contributions due to single defect jumps, cascades, and vacancy emission as: D(n) = Ds (n) + Dc (n) + De (n) ,

(8.67)

where 3n1/3 [Dv (Cv − Cv0) + DiCi ] , 2a2 + 2, + , Kieff Ndi2 3n2/3 Kveff Ndv c + , D (n) = 4a kv Ndv ki Ndi Ds (n) =

De (n) =

9DvCv0 n2/3 , 2a2

(8.68) (8.69) (8.70)

8.1 Void Nucleation

/

363

0

2 and K eff j is the effective generation rate of free point defects, Nd j and Nd j are the average number and the average square number of free point defects generated in a single cascade, respectively, and k2j is the total sink strength for point defects of the type j. The solution to the general kinetic equation is similar to that for the case of interstitial clusters and is given in [14]. For the case of small critical vacancy size, the solution is: 1/2 β (DvCv − DiCi ) ∼ Pm = (n0 − nv 0 ) 1/3 6π Rcr ncr DiCi (1 + dncr ) 2/3 2/3 η (β /Rcr )ncr − n0 × exp − , (8.71) 1/3 1 + 1/(d encr ) + d c /d e

where n0 is the initial void embryo size (generally ∼ 4 vacancies), nv0 is a minimum size of a void embryo below which it is no longer a void (generally ∼ 2–3 vacancies), d = d c + d e , β = 2γΩ /kT and Rcr and ncr are the size and vacancy content of the critical size embryo. The term Rcr is determined from Eqs. (8.65) and (8.66) under that condition that a void will grow if it receives a net vacancy flux (DvCv > DiCi ): Rcr =

β DvCvV , DvCv − DiCi − DvCvV

(8.72)

and R(n) = an1/3. The terms d c and d e are strengths of the diffusive spread for clusters and for vacancy emission relative to single point defects: dc =

Dc (ncr ) 1/3 s ncr D (ncr )

,

de =

De (ncr ) 1/3 s ncr D (ncr )

,

(8.73)

and the function η has a value between 0.55 and 0.84. Application of Eq. (8.71) for various values of d c and d e and for a void embryo size of 4 vacancies leads to nucleation probabilities in the range 10−6 to 10−4 for critical vacancy clusters of size ∼ 100 vacancies (Fig. 8.12). The nucleation rate is then: J∼ =

Kcleff Pm , Nd

(8.74)

where Kcleff is the effective generation rate of point defects in cluster and free form and Nd is the average total number of point defects generated in a single cascade and εi is the fraction of interstitials produced in cascades in the form of immobile clusters. Figure 8.13 shows the void nucleation rate calculated for annealed copper compared with experimental data at 250, 300 and 350 ◦C and different surface energies, γs and for different values of d e . In terms of void nuclei created cm−3 s−1 , the nucleation rate is in the range 1015 to 1018, which is larger than what was predicted by conventional nucleation theory. Thus, the effect of production bias is to increase the nucleation rate.

364

8 Irradiation-Induced Voids and Bubbles

Fig. 8.12. Nucleation probability plotted from Eq. (8.71) for initial void size of four vacancies and minimum size of one vacancy and for different values of d c and d e vs. the critical void (DvCv − DiCi )[1 − exp(−β /Rcr )] size, ncr . The term ν = (after [14]) DiCi

Fig. 8.13. Void nucleation rate vs. irradiation temperature for the case of copper under a displacement rate of 10−8 dpa/s (after [14])

8.2 Void Growth

365

8.2 Void Growth Having determined expressions for the rate at which voids are nucleated in the solid, we now turn to determining the rate at which the void nuclei grow into stable voids. As mentioned earlier, we will assume that the nucleation and growth stages are separated in time and that only when the void embryos are established does growth begin. Of course, this is a simplification of the true in-reactor situation in which the growth of stable nuclei is occurring simultaneously with nucleation. Void growth is determined by solving the point defect balance equations developed in Chap. 5. These equations provide the vacancy and interstitial supersaturations that drive the nucleation and growth processes. The concentrations of vacancies and interstitials in the solid are determined by equating the rates of defect production and removal by all mechanisms. By doing so, the time derivatives are removed and the resulting solution has the form of a steady state solution. However, since the defect concentrations are changing with time (dose), the steady state solution is valid over only short time periods, and is termed quasi-steady state. The quasi-steady state solution has value because the changes in sink strength due to microstructure evolution is slow compared to the response time of the defect populations. So in essence, the problem can be solved by assuming an initial condition that properly characterizes the sink strengths, solving the point defect balance equations for those sink strengths, then updating the sink strengths and iterating. Rates of production and removal are assumed to be uniform throughout the metal. Clearly, strong gradients will exist close to the sink. But they can be neglected by homogenizing or smearing the sink strengths, that is, by replacing discrete sinks by spatially uniform absorbers of point defects so that the aggregate effect on defect absorption is the same in the homogenized sink case as in the heterogeneous sink case. The sink strengths are those described in Chap. 5. Void growth is then calculated according to rate theory as developed by Brailsford and Bullough [14] subject to the following simplifications: 1. Discrete sinks are replaced by a continuous or smeared distribution of sinks. 2. Each sink is given a strength so that the current of defects to the smeared sink is the same as the current to the actual sinks in the real material. 3. Steps 1 and 2 remove the spatial dependence of Cv and Ci and the point defect balance equations become:

∂ Cv = K0 − ∑ Avj − Riv ∂t j ∂ Ci j = K0 − ∑ Ai − Riv , ∂t j

(8.75)

where the first term on the right is the production rate of vacancies and interstitials, the second term is the loss rate to all sinks and the last term is the loss rate due to vacancy–interstitial recombination. 4. Vacancy and interstitial concentrations, Cv and Ci are calculated from Eq. (8.75). The change in sink strength due to the flow of defects to the sink is calculated,

366

8 Irradiation-Induced Voids and Bubbles

and the process, starting with step 1, is iterated in order to advance in time and dose. Reaction rate constants for defect–sink reactions and sink strengths for the relevant sinks were determined in Chap. 5 and summarized in Table 5.1. Recall that sinks are classified as neutral (voids, grain boundaries, incoherent precipitates), biased (dislocation network and dislocation loops) or variable biased (coherent precipitates and over/undersized solutes). For all sink types, the defect absorption rate is proportional to the diffusion coefficient of the point defect and the difference in defect concentration between the bulk and the sink surface. With the exception of dislocation loops, the interstitial concentration at the sink surface is insignificant compared to the bulk value and may be neglected. In the case of vacancies, their concentration at the network dislocation core is maintained at the equilibrium concentration. For voids and loops, the vacancy concentration at the sink surfaces must also be determined. Once the sink strengths and the defect concentrations at the sink surfaces are all known, then we can determine the net absorption rate of defects by void nuclei and use this information to determine the growth rate of the voids. 8.2.1 Defect Absorption Rates and Concentrations at Sink Surfaces We seek to determine expressions for the absorption rates of defects for each of the relevant of sinks, categorized according to sink type. The general form of the absorption rate is: AXj = kX2 D j (C j − CXj ) = kX2 D jC j − LXj ,

(8.76)

where AXj is the absorption rate of defect j by sink X, kX2 is the strength of sink X, D j is the diffusion coefficient of defect j, C j and CXj are the bulk concentration and sink surface concentration of defect j, and LXj is the thermal emission rate of defect j by sink X. Note that for neutral sinks, the sink strengths are dependent only on the character of the sink and not the defect. This is the advantage of writing the loss terms using sink strengths rather than reaction rate constants. Neutral Sinks The loss rate of point defects to voids can be written as: 2 V 2 V AV v = kV Dv (Cv − Cv ) = kV DvCv − Lv V 2 Ai = kV DiCi ,

(8.77)

2 is the sink strength of a void given in Table 5.1, CvV is the vacancy concenwhere kV tration at the void surface, LV v is the thermal emission rate of vacancies at the sink surface and all voids are assumed to be the same size. The loss rate of defects to incoherent precipitates is: 2 AIP v = kIP DvCv 2 AIP i = kIP DiCi ,

(8.78)

8.2 Void Growth

367

and to grain boundaries the rate is: 2 Agb v = kgb DvCv gb

2 Ai = kgb DiCi ,

(8.79)

where the sink strengths are given in Table 5.1, and thermal emission terms have been neglected. Among Eqs. (8.77), (8.78), and (8.79), the term that is yet to be determined is the vacancy concentration at the void surface, CvV . This is done as follows. Recall from Eq. (4.14) that the thermal equilibrium concentration of vacancies in a solid is: Sf Hf 1 0 exp , Cv = exp Ω k kT where Hf = Ef + pΩ ,

(8.80)

and the pΩ term was neglected for single vacancies embedded in the lattice. This simplification does not hold in the solid surrounding a void where forces such as surface tension, pressure due to gas in the void and an external hydrostatic stress are acting. For example, the existence of a void surface produces a surface tension that can be determined, using Fig. 8.14, as follows: 2π rγ sin θ ∼ 2π rγ 2π r γ r 2γ Force = = , (8.81) θ = = unit area A π r2 π r2 R R where the approximation is that sin θ is replaced with θ for small θ . Hence, the p term in Eq. (8.80) becomes: 2γ , (8.82) R where the minus sign enters because the surface tension acts in an inward direction to shrink the void. The vacancy concentration at the void surface then becomes: Sf 1 Ef pΩ V Cv = exp exp − exp − , (8.83) Ω k kT kT p=−

where: Cv0 =

Sf 1 Ef exp exp − , Ω k kT

and substituting for pΩ from Eq. (8.82) gives: 2γΩ CvV = Cv0 exp , RkT and Eq. (8.77) becomes:

2γΩ V 2 0 Av = kV Dv Cv − Cv exp . RkT

(8.84)

(8.85)

(8.86)

368

8 Irradiation-Induced Voids and Bubbles Fig. 8.14. Schematic of the surface tension on a void of radius r

Biased Sinks The defect loss rate to network dislocations is given by: 2 2 Adv = kvd Dv (Cv − Cv0 ) = kvd DvCv − Ldv 2 Adi = kid DiCi ,

(8.87)

where the sink strengths are given in Table 5.1 and the term Cv0 is the thermal equilibrium concentration of vacancies. For interstitial dislocation loops, the loss term is: 2 2 Dv (Cv − CvL ) = kvL DvCv − LLv ALv = kvd 2 2 ALi = kid Di (Ci − CiL ) = kiL DiCi − LLi ,

(8.88)

where the sink strengths are the same as for network dislocations since the dislocation core is the same. However, the defect concentration at the sink surface is different from the thermal equilibrium value because addition of a vacancy or an interstitial to the dislocation loop contracts or expands, respectively, the size of the loop and this requires a change in energy. The concentration of vacancies and interstitials in equilibrium with a loop are CvL and CiL , respectively. Following the analysis in [4] the defect concentration in equilibrium with the loop is determined by considering the Gibbs free energy of a piece of metal containing nv vacancies and ni interstitials at concentrations CvL and CiL , and a single interstitial loop containing mi interstitials: G = G0 + EL(mi ) + nv μv + ni μi ,

(8.89)

where G0 is the free energy of solid without the loop but with Cv and Ci defects, EL (mi ) is the energy of the loop, and μi,v are the chemical potentials of interstitials and vacancies in the solid. For the system to be in chemical equilibrium, the transfer of point defects between the solid and the loop must cause no change in the free energy of the system: dEL δG = δ mi + μ v δ n v + μ i δ n i = 0 , (8.90) dmi

8.2 Void Growth

369

and

δ mi = δ n v − δ n i ,

(8.91)

since the number of interstitials in the loop must come from the bulk. Eliminating δ mi from Eqs. (8.91) and (8.92) gives: dEL dEL δ nv − δ n i + μv δ n v + μi δ n i = 0 . (8.92) dmi dmi Since changes in vacancy and interstitial concentrations are arbitrary and independent of each other, the coefficients of both changes are set equal to zero, leading to: dEL + μv = 0 dmi dEL − μi = 0 . dmi

(8.93)

From Eq. (8.12), the chemical potential of vacancies and interstitials in a solid with concentrations CvL and CiL is:

μv = kT ln

CvL Cv0

CL μi = kT ln i0 . Ci

(8.94)

For vacancies and interstitials in equilibrium: CvLCiL = Cv0Ci0 ,

(8.95)

or from Eq. (8.94):

μv = − μi .

(8.96)

Combining Eqs. (8.93) and (8.94) for vacancies and then for interstitials, yields: dEL / dmi L 0 Cv = Cv exp − kT (8.97) dE / dmi L L 0 Ci = Ci exp . kT Using Eq. (7.62) for the energy of a Frank loop: √ 1/2 √ 3a2 mi 3a2 mi 2 +π γSFE , EL = 2 π μ b 4π 4π

370

8 Irradiation-Induced Voids and Bubbles

and dropping the second term for simplicity, then dEL / dmi becomes:

Θ dEL = √ , dmi 2 mi √ 1/2 3a2 2 . Substituting into Eq. (8.97) yields: where Θ is 2π μ b 4π Θ L 0 Cv = Cv exp − √ 2 mi kT Θ L 0 Ci = Ci exp √ . 2 mi kT

(8.98)

(8.99)

Note that the vacancy concentration in equilibrium with an interstitial loop is less than the equilibrium vacancy concentration in the solid while the reverse is true for interstitials. The absorption rates of vacancies and interstitials at loops then becomes, from Eq. (8.88):

Θ L 0 Av = zv Dv ρL Cv − Cv exp − √ 2 mi kT

(8.100) Θ L 0 Ai = zi Di ρL Ci − Ci exp √ . 2 mi kT Variable Biased Sinks The sink strengths for variable biased sinks are given in Eq. (5.117) and are: 2 = 4π RCP ρCPYv kvCP 2 kiCP = 4π RCP ρCPYi ,

where Yv,i are sink strengths for coherent precipitates for vacancies and interstitials and the loss rate of point defects to coherent precipitates is: 2 ACP v = kvCP DvCv = 4π RCP ρCPCvYv 2 ACP i = kiCP DiCi = 4π RCP ρCPCiYi .

(8.101)

8.2.2 Point Defect Balances Now that we have expressions for the absorption rates of defects for each type of sink, we can construct the steady state, point defect balances for the solid under irradiation: K0 − ∑ Avj − Riv = 0 j

K0 − ∑ Aij − Riv = 0 , j

(8.102)

8.2 Void Growth

371

and in the most general form: K0 − kv2 Dv (Cv − CvX ) − KivCvCi = 0

(8.103)

K0 − ki2 Di (Ci − CiX ) − KivCvCi = 0 , where kv2 and ki2 are the total sink strengths for vacancy and interstitial loss: 2 2 2 2 2 2 + kvIP + kvgb + kvN + kvL + kvCP kv2 = kvV

(8.104)

2 2 2 2 2 2 ki2 = kiV + kiIP + kigb + kiN + kiL + kiCP ,

and the CvX and CiX are concentrations of vacancies and interstitials at the sink surface. Now, since defect production rates and recombination rates in Eq. (8.103) are equal and there is no net accumulation of point defects at coherent precipitates, then:

∑ Avj = ∑ Aij , j

(8.105)

j

or gb

IP gb d L V IP d L AV v + Av + Av + Av + Av = Ai + Ai + Ai + Ai + Ai ,

(8.106)

and therefore: 2 2 2 2 2 2 N L + kvIP + kvgb + kvN + kvL + kvCP )DvCv − LV (kvV v − Lv − Lv 2 2 2 2 2 2 = (kiV + kiIP + kigb + kiN + kiL + kiCP )DiCi − LLi .

(8.107)

where the L terms are the thermal emission of the defect from the sink. Substituting in for the expressions for sink strength and thermal emission from the respective equations in Chaps. 5 and 7 gives:

2γΩ 0 + zv ρN Dv Cv − Cv0 + 4π RCPρCP DvCvYv 4π RV ρV Dv Cv − Cv exp RkT

Θ 0 + zv ρL Dv Cv − Cv exp − √ 2 mi kT = π RV ρV DiCi + zi ρN DiCi + 4π RCPρCP DvCvYi

Θ 0 + zi ρL Di Ci − Ci exp √ , 2 mi kT (8.108) where terms for grain boundaries and incoherent precipitates are neglected for simplicity. Since the thermal equilibrium interstitial concentration, Ci0 is extremely small, the thermal emission of interstitials from loops can be neglected.

372

8 Irradiation-Induced Voids and Bubbles

8.3 Void Growth Equation Now that we have determined the absorption rate of defects for each sink in the solid, we focus on the void with the objective of developing an expression describing its rate of growth. The void growth equation has its origins in the net flux of vacancies to a void embryo. The net rate of absorption of vacancies by a void is: V V V V AV , (8.109) net = Av − Ai = 4π RDv Cv − Cv − 4π RDi Ci − Ci where R = void radius (we have dropped the subscript V for simplicity) Cv,i = vacancy/interstitial concentration in the solid CvV = vacancy concentration at the void surface, and thermal emission of interstitials from loops is neglected The rate of change in volume of the void is just the net absorption rate times the defect volume, Ω : dV = 4π RΩ Dv Cv − CvV − DiCi , dt

(8.110)

and since, 4 V = π R3 , 3

(8.111)

we obtain the common form of the void growth equation: dR Ω = R˙ = Dv Cv − CvV − DiCi . dt R

(8.112)

Our objective is to determine an expression for the void growth equation, which amounts to determining the values for Cv ,Ci , and CvV . The general solution procedure is thus to solve the point defect balance equations in Eq. (8.75) for Cv and Ci at some initial value of the void radius, R(0) and then to use those values of Cv and Ci in Eq. (8.112) to increment the void size from R to R . Since sink strength changes with void size, updated values of Cv and Ci must be obtained for the next void growth increment. The process is then iterated to describe the change in void size with time or dose. This process can be carried out numerically and with small time steps in order to minimize the time increment over which the sink strengths are assumed to be constant. In solving for void size in this way, changes to the microstructure can also be incorporated at the time step boundaries. While a numerical solution of the void growth equation will produce the most accurate result, it provides no insight into the governing processes during void growth. Brailsford and Bullough [15] inserted the solution of Eq. (8.75), into Eq. (8.112) to obtain an approximate analytical result that provides an excellent tool for understanding the parameters governing void growth. Mansur [5, 16] advanced the analysis to develop expressions for the dependence on critical parameters affecting void growth. We begin by returning to the point defect balance equations

8.3 Void Growth Equation

373

at steady state in order to determine the bulk concentrations of vacancies and interstitials, Cv and Ci . Setting the time rate of change of the vacancy and interstitial concentrations equal to zero in Eq. (8.75) gives: K0 − ∑ Avj − Riv = 0 j

K0 − ∑ Aij − Riv = 0 ,

(8.113)

j

or K0 − KivCiCv − KvsCvCs = 0 K0 − KivCiCv − KisCiCs = 0 ,

(8.114)

with solutions:

2 C2 1/2 K0 Kvs Kvs −KisCs s + + 2Kiv Kiv Kis 4Kiv

1/2 K 2 C2 K0 Kis −KvsCs Ci = + + is s , 2Kiv Kiv Kvs 4Kiv

Cv =

(8.115)

where Cs is the sink concentration. Using Table 5.1 to write the reaction rate constants for vacancies and interstitials at sinks as sink strengths gives:

1/2 −ki2 K0 kv2 Di kv2 D2v + + 2Kiv Kiv ki2 Dv 4Kiv

1/2 K0 ki2 Dv ki2 D2i −kv2 Ci = + + . 2Kiv Kiv kv2 Di 4Kiv

Cv =

(8.116)

Defining:

η=

4Kiv K0 , Di Dv kv2 ki2

(8.117)

and kv2 = zv ρd + 4π RρV + 4π RCPρCP ki2 = zi ρd + 4π RρV + 4π RCPρCP ,

(8.118)

where, for simplicity, we have neglected grain boundaries, incoherent precipitates and bias factors on voids and coherent precipitates, and the network dislocations and dislocation loops are represented by a single term with density ρd = ρN + ρL . Using Eqs. (8.117) and (8.118), then Eq. (8.116) can be written as: Di ki2 (η + 1)1/2 − 1 Cv = 2Kiv (8.119) Dv kv2 1/2 (η + 1) − 1 . Ci = 2Kiv

374

8 Irradiation-Induced Voids and Bubbles

The void growth rate from Eq. (8.112) can be written in the form: R˙ = R˙ 0 X(η ) ,

(8.120)

where K0 (zi − zv )ρd Ω R(zv ρd + 4π RρV)

. R˙ 0 = (zi − zv )ρd zi ρd + 4π RρV + 4π RCPρCP 1 + zv ρd + 4π RρV

(8.121)

Equation (8.121) can be simplified by dropping the last term in the square brackets in the denominator, since the difference (zi − zv ) is small, giving: R˙ 0 =

K0 (zi − zv )ρd Ω . R(zv ρd + 4π RρV)(zi ρd + 4π RρV + 4π RCPρCP )

(8.122)

This growth term is independent of temperature and is proportional to the dislocation bias for interstitials (zi − zv ) and the defect production rate. Note that R˙ 0 is: – – –

Independent of temperature Proportional to the dislocation bias (zi − zv ) Proportional to the defect production rate, K0

The term X(η ) is given by: X(η ) = F(η ) − 2ζ ,

(8.123)

where: F(η ) =

2 (η + 1)1/2 − 1 , η

(8.124)

and η is a dimensionless parameter defined in Eq. (8.117). Substituting Eq. (8.123) into Eq. (8.120) gives: R˙ = R˙ 0 F(η ) − 2R˙ 0 ζ .

(8.125)

The quantity η in the function F(η ) can be simplified by substituting in for kv2 and ki2 from Eq. (8.104) (or Table 5.1), giving:

η=

4Kiv K0 . (8.126) Di Dv (zi ρD + 4π RρV + 4π RCPρCP )(zv ρd + 4π RρV + 4π RCPρCP )

Using the approximation that zi ∼ = zv , and eliminating Kiv by using Eq. (5.57) gives:

η=

4ziv K0 Ω . Di Dv (zρD + 4π RρV + 4π RCPρCP )2

(8.127)

The expression for η is substituted into Eq. (8.124) to obtain an expression for F(η ). This function describes the effect of homogeneous recombination on void growth

8.3 Void Growth Equation

375

(Fig. 8.15). When recombination is negligible Kiv → 0 and η → 0, and F → 1, or lim F(η ) = 1. η →0

Turning now to the second term in Eq. (8.125), we define for simplicity: R˙ th = −2R˙ 0ζ ,

(8.128)

so that Eq. (8.125) can now be written as: R˙ = R˙ 0 F(η ) + R˙ th ,

(8.129)

The term ζ is a function of temperature and is expressed as:

ζ = ζ (T ) =

Dv (zv ρd + 4π RρV) [zi ρd + 4π (RρV + RCP ρCP )] 2K0 (zi − zv ) [zv pd + 4π (RρV + RCP ρCP )] (8.130) ) V V * V 0 L × 4π RCPρCPCv + zv ρN Cv − Cv + ρL Cv − Cv .

so that: −2Dv (zv ρd + 4π RρV) [zi ρd + 4π (RρV + RCP ρCP )] R˙ th = −2R˙ 0 ζ = 2K0 (zi − zv )ρd [zv ρd + 4π (RρV + RCP ρCP )] K0 (zi − zv )ρd Ω R(zv ρd + 4π RρV)

× (zi − zv )ρd zi ρd + 4π RρV + 4π RCPρCP 1 + zv ρd + 4π RρV × 4π RCP ρCPCvV + zv ρN CvV − Cv0 + ρL CvV − CvL .

(8.131)

By approximating zi ∼ = zv , numerous terms in Eq. (8.131) cancel, leaving: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP ) × 4π RCP ρCPCvV + zv ρN CvV − Cv0 + ρL CvV − CvL .

(8.132)

Fig. 8.15. The behavior of the function F(η ) in Eq. (8.124) as a function of η

376

8 Irradiation-Induced Voids and Bubbles

Substituting in for CvV and CvL from Eqs. (8.85) and (8.99), respectively, gives: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 2γΩ × 4π RCP ρCPCv0 exp + zv ρN Cv0 exp − Cv0 (8.133) RkT RkT 2γΩ Θ +ρL Cv0 exp − Cv0 exp − √ . RkT 2 mi kT

Approximating exp (x) ∼ x + 1 for small x, in the exponential terms of Eq. (8.133) gives: R˙ th =

−Dv Ω R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 0 × 4π RCP ρCPCv exp RkT

2γΩ 2γΩ Θ 0 + ρL + √ +zvCv ρN , RkT RkT 2 mi kT

(8.134)

and pulling the term Cv0 out into the coefficient yields: R˙ th =

−Dv Ω Cv0 R(zi ρd + 4π RρV + 4π RCPρCP )

2γΩ 2γΩ A 2γΩ × 4π RCP ρCP exp + zv ρL + √ + zv ρN , RkT RkT RkT 2 mi kT (8.135)

which is the simplified expression for the thermal emission term. This term represents the thermal emission of defects from sinks. It is independent of defect production rate and is strongly temperature-dependent. Note that at very low temperature, R˙ th → 0, because of the terms Dv and Cv0 . ˙ determined from Eq. (8.120), The rate of change in the void radius with time, R, can be used to determine the volumetric swelling rate: dV = 4π R2 R˙ . dt

(8.136)

Void swelling can be represented in terms of the void size distribution as follows. If ρV (R) dR is the number of voids/cm3 with radii between R and R + dR, then the total void number density is:

ρV =

∞ 0

ρV (R) dR ,

(8.137)

the average void size is: R=

1 ρV

∞ 0

RρV (R) dR ,

(8.138)

8.3 Void Growth Equation

377

and the amount of void swelling is defined by the change in volume of the solid: 4 ΔV = π V 3

∞ 0

R3 ρV (R) dR .

(8.139)

If the void distribution is narrow, then we can approximate the integral in Eq. (8.139) with: ΔV 4 3 = π R ρV . V 3

(8.140)

The equations provided in this section allow the determination of the rate of growth of voids in a solid under irradiation, and consequently, the rate of swelling of that solid. The following sections address the effects of various parameters on void growth. 8.3.1 Temperature Dependence Figure 8.16 provides a typical plot of void swelling as a function of temperature. Note that swelling is characterized by a peak at intermediate temperature. This behavior should look familiar from the temperature dependence of RIS since the origin is essentially the same. Low defect mobility limits void growth at low temperature, and the approach of the defect concentration to the thermal equilibrium value, and hence the loss of supersaturation, limits void growth at high temperature. In the preceding analysis of the void growth equation, the two highly temperature sensitive parameters are the vacancy diffusion coefficient Dv and the equilibrium vacancy concentration Cv0 . The temperature dependence of the term R˙ 0 F(η ) is contained in the parameter η , which is controlled by Dv . At low temperatures, swelling is low because vacancies are practically immobile. A low value of Dv makes η large and forces F to become small, resulting in a low value for the term R˙ 0 F(η ). The term R˙ th approaches zero since it is proportional to DvCv0 . Since both F (η ) and R˙ th become small at low temperature, void growth ceases. Under these conditions, the concentration of vacancies builds up and vacancies and interstitials are lost to recombination. At high temperature, the emission of vacancies by voids counterbalances the net vacancy influx driven by irradiation and suppresses swelling. When in the void growth equation η becomes small and F approaches unity, the term R˙ th also increases (but in the negative direction) and dominates at the highest temperatures. Hence a maximum in the growth rate is predicted at intermediate temperature where both thermal emission and mutual recombination are less important and the net flow of vacancies to voids is maximized. Figure 8.17 shows how the components of the void growth rate combine to result in a peak at intermediate temperature. This is found to be true with all metals. Figure 8.18a shows an example of the sharp dependence of void swelling on temperature in an Fe–Cr–Ni alloy irradiated in the BN-350 reactor as a function

378

8 Irradiation-Induced Voids and Bubbles

Fig. 8.16. Swelling in nickel as a function of irradiation temperature for a fluence of 5 × 1019 n/cm2 (after [17])

Fig. 8.17. Construction of the total void swelling rate R˙ from its components R˙ 0 F and R˙ th

of dose and temperature. All the data were for irradiation over a fixed time period, reflecting the variation of dose rates with position in the core. Closed symbols represent samples in which voids were found and open symbols were samples that exhibited no voids. Note that despite the differing doses and dose rates, void nucleation occurs with a very sharp temperature threshold at about 302 – 307 ◦C, illustrating the high sensitivity of void formation to temperature. The gen-

8.3 Void Growth Equation

379

Fig. 8.18. (a) Dosetemperature plot of swelling in a Fe–Cr–Ni alloy irradiated in the BN350 fast reactor showing the sharp temperature threshold for swelling (after [18]). (b) Schematic of the temperature dependence of void density and void size

eral behavior of the void number density and size with temperature is shown in Fig. 8.18b. With increasing temperature, the void density falls logarithmically and the size increases, which is the typical behavior for a process that is dominated by nucleation at low temperatures where the void growth is slow, and by growth at high temperature where the free energy difference driving void growth is small. Figure 8.19 shows images of the microstructure in a baffle bolt used to secure baffle former plates against the baffle in a pressurized water reactor. In this case, the head was closest to the core (received the highest dose), and was exposed to the coolant, hence the lowest temperature. Gamma heating caused the temperature to exceed the coolant temperature (∼ 320 ◦C) along the length of the bolt. While the

380

8 Irradiation-Induced Voids and Bubbles

Fig. 8.19. Swelling in a cold-worked 316 SS baffle bolt in a PWR as a function of position along the bolt length. The bolt head was closest to the core and the temperature distribution is caused by a combination of gamma heating and whether the bolt was exposed to the coolant (courtesy S.M. Bruemmer and Garner FA, PNNL)

doses differ somewhat, the dominant influence of temperature is noted by both the lack of voids in the lowest temperature location (head) and the largest void size at the highest temperature (top shank). 8.3.2 Dose Dependence Understanding how swelling depends on dose is critical in the design and operation of components in radiation environments in which voids have the potential to form and grow. From the discussion in the previous section, the dependence is complicated by the occurrence of the defect production rate, K0 , in the terms R˙ 0 and F(η ). So we will take a different approach in determining the void growth rate dependence on dose, following that of Mansur [5]. Recall the expressions for Cv and Ci given in Eq. (8.119): Di ki2 (η + 1)1/2 − 1 2Kiv Dv kv2 (η + 1)1/2 − 1 , Ci = 2Kiv

Cv =

8.3 Void Growth Equation

381

and for η as given in Eq. (8.117):

η=

4Kiv K0 . Di Dv kv2 ki2

We can write the term in brackets in Eq. (8.119) as: 1/2 4K K iv 0 1+ −1 . (η + 1)1/2 − 1 = Di Dv kv2 ki2 Then, DvCv and DiCi can be written as: Dv Di ki2 zv 4Kiv K0 1/2 DvCv = −1 1+ 2Kiv Di Dv kv2 ki2 Dv Di kv2 zi 4Kiv K0 1/2 DiCi = −1 . 1+ 2Kiv Di Dv kv2 ki2 Neglecting thermal emission, and substituting into Eq. (8.112) gives: 1/2 4K Ω D D K v i iv 0 1+ − 1 (kv2 zv − ki2 zi ) . R˙ = 2RKiv Di Dv kv2 ki2

(8.141)

(8.142)

(8.143)

Substituting for kv2 and ki2 from Eq. (8.104) and considering only coherent precipitates, network dislocations and loops gives: 1/2 Ω D D K 4K v i iv 0 −1 1+ R˙ = 2RKiv Di Dv kv2 ki2 L N CP L N × 4π RCP ρCP zCP . i zv − zv zi + ρL zi zv − zv zi + ρN zi zv − zv zi (8.144) Simplifying Eq. (8.144) for the case of voids and total dislocation density only, we have: 1/2

Ω D D K 4K v i iv 0 (8.145) R˙ = − 1 ρd zdi zv − zdv zi . 1+ 2 2 2RKiv Di Dv k v k i The term zdi zv − zdv zi is the bias of dislocations vs. that for voids and is the determinant of the propensity for a void to grow or shrink. Growth will occur if zdi zv > zdv zi , zd zv and shrinkage will occur if the inequality is in the other or stated as ratios, id > zv zi direction. The presence of other sinks will affect swelling through their inclusion in the terms kv2 and ki2 . The larger the sink strengths, the lower will be the void growth rate due to the loss of defects to those sinks.

382

8 Irradiation-Induced Voids and Bubbles

The limiting behaviors of Eq. (8.145) are the cases in which recombination dom4Kiv K0 inates

1 (loss of defects to recombination is much larger than that lost Di Dv kv2 ki2 4Kiv K0 to sinks) and loss to sinks dominates 1 [5]. Assuming that the only Di Dv kv2 ki2 sinks besides voids are network dislocations, we have: 1/2 1/2 Ω Di Dv K0 1/2 Qi Qv zNi zv − zNv zi ˙ R= : recombination dominant R zNi zNv Kiv (1 + Qv)1/2 (1 + Qi)1/2 (8.146) N Ω K0 Qi Qv R˙ = z zv − zNv zi : sink dominant , RρN (1 + Qv)(1 + Qi ) i (8.147) where: Qi,v =

zNi,v ρN 4π Rρvzi,v

(8.148)

is the ratio of dislocation sink strength to void sink strength. Note that the growth 1/2 rate is dependent on K0 when recombination is dominant, Eq. (8.146). However, when sinks are dominant, Eq. (8.147) shows that the growth rate is proportional to K0 . Multiplying Eq. (8.147) by 4π R2ρV and given that Ω = 1/N0 , the site density, gives the volume swelling rate: zi − zv Q d(ΔV /V ) = K0 . (8.149) dt zv (1 + Q)2 This is the same expression that can be obtained from Eq. (8.122) by neglecting the effect of coherent precipitates. For Q = 1 and zi − zv = 0.01, we have: ΔV ∼ % = 1/4 × (dose in dpa) . V

(8.150)

Garner [19] has shown that over a wide dose range, the steady state swelling rate is of the order of ∼ 1%/dpa (Fig. 8.20). The linear dependence is consistent with a sink-dominated process, but the magnitude of the coefficient is a factor of four greater than that predicted by Eq. (8.150). The discrepancy is likely due to the effect of clusters that is not accounted for in the rate theory model. A closer look at the behavior of vacancies and interstitials in the cascade shows that the fraction of vacancies and interstitials that form clusters is larger than has been accounted for thus far. Vacancy clusters form near the cascade core and interstitial clusters form near the cascade periphery. Mobile interstitial clusters can reach sinks by migration of the cluster as a whole. Vacancies emitted by vacancy clusters by thermal emission are also free to reach sinks. Since the fraction of interstitials and vacancies in clusters is not the same, nor is their thermal stability, the difference between vacancy and interstitial clusters results in a difference in the effective production rates of vacancies

8.3 Void Growth Equation

383

Fig. 8.20. (a) Early development of 1%/dpa swelling rates in aged OKH16N15M3B steel during irradiation in the BOR-60 reactor at 400 – 550 ◦C (after [20]). (b) Variations in swelling at 540 ◦C in EBR-II for two nominally similar heats of 316 stainless steel as a function of starting condition (after [21])

compared to that of interstitials, termed the production bias, and can influence void swelling. The net result is that the sink strength of the clusters is much greater than that of the measurable dislocation loops, resulting in a much greater driving force for void swelling than is accounted for by the rate equation formulation. This is one of the reasons that the observed steady state swelling dependence on dose is greater than that predicted by the rate equation formulation.

384

8 Irradiation-Induced Voids and Bubbles

8.3.3 Role of Dislocations as Biased Sinks The dislocation structure of an alloy can exert a profound effect on the swelling behavior. Equation (8.122) demonstrates that both a biased sink (e.g., dislocations) and a neutral sink are necessary for void growth. If the bias was removed, zi = zv , then R˙ 0 = 0 and swelling will not occur as defects will flow equally to each sink. The Q-dependence of R˙ 0 is shown in Fig. 8.21. Note that R˙ 0 is a maximum at Q = 1, or when the flow of vacancies to voids and dislocations is equal. The regime Q < 1 is representative of the low dose regime in which both R and ρV are small, so vacancy loss to the existing dislocation network dominates. This is why cold-worked alloys swell less. When Q ∼ 1, then the flow of vacancies to voids and dislocations is approximately equal. This is the regime where bias exerts its greatest influence. If the flow of vacancies and interstitials to sinks is equal, and more interstitials go to dislocations, then more vacancies must flow to voids. At Q ∼ 1, the flows are equal so the bias is most effective in promoting void growth. When Q > 1, defect flow to voids dominates the loss terms and since few defects flow to dislocations, the bias is not very effective in creating an imbalance in point defect fluxes, so the flow of vacancies and interstitials to voids is similar in magnitude and void growthslows orceases. Although dislocations exhibit βd ≥ 1 , in a cold-worked material, the disloa slight preference for interstitials βV cations provide so many sinks for vacancies that the effect of a vacancy supersaturation is essentially multiplied, resulting in low void nucleation and growth rates. By the same mechanism, grain boundaries provide unbiased sinks for point defects and will keep the vacancy supersaturation too low for growth provided the grain boundary area is large enough (i.e., very small grains). Figure 8.22 shows a plot of swelling rate vs. the sink strength ratio, Q for several austenitic stainless steels and verifies that indeed, the dependence shown in Fig. 8.21 is obeyed in practice. The effect of cold-work on swelling in reactor exposures is shown in Fig. 8.23. Figure 8.23a shows the effect of cold-work on swelling in 316 stainless steel ir-

Fig. 8.21. Dependence of swelling on the dislocation/void sink strength ratio, Q in Eq. (8.149)

8.3 Void Growth Equation

385

Fig. 8.22. Experimentally observed swelling rates as a function of Q for austenitic stainless steels (after [5])

radiated in EBR-II at 650 ◦C to levels of 33 and 50 dpa. Note that for both cases, the amount of swelling decreases with increasing cold-work. Figure 8.23b shows that cold-work affects the temperature dependence of swelling by suppressing the magnitude of the swelling peak with increasing levels of cold-work. The data are taken from a stainless steel irradiated to doses of 20 – 61 dpa in the RAPSODIE reactor. Figure 8.23c shows the effect of cold-work on the dose dependence of swelling in 304 stainless steel, and that increasing cold-work decreases the amount of swelling, but at reduced rates as the amount of cold-work increases. Note also that these data show that the primary effect of cold-work is to extend the transient swelling regime, rather than to alter the steady state swelling rate. 8.3.4 Dose Rate Dependence The location of the peak swelling temperature depends on the dose rate, sink strength and the predominant mode of defect loss. When the dose rate increases, more point defects are created, but their migration velocities are unchanged. To remove defects at the higher rate at steady state requires point defect concentrations to be higher, resulting in greater recombination and a reduction in the net absorption of vacancies by voids, and hence, a reduction in the void growth rate. As a result,

386

8 Irradiation-Induced Voids and Bubbles

Fig. 8.23. (a) Effect of cold-work level on the swelling of 316 stainless steel irradiated at 650 ◦C in EBR-II to 33 and 50 dpa (after [22]). (b) Dependence of swelling on cold-work for various temperatures for 316 stainless steel irradiated in the RAPSODIE reactor to doses of 20 – 71 dpa (after [23]). (c) Effect of cold-work on swelling in 304 stainless steel at 450 ◦C in EBR-II (after [24])

8.3 Void Growth Equation

387

the bell-shaped swelling curve is displaced to higher temperatures with increasing dose rate. Figure 8.24 is a plot of the temperature dependence of the term F(η ) in Eq. (8.125), and illustrates the shift of the swelling peak with dose rate, K0 . Alternatively, at a given temperature, the void growth rate decreases for increasing dose rate. At temperatures where thermal emission is non-negligible, the void growth rate is a complicated function of dose rate. Nevertheless, the experimental data substantiate the effect of dose rate on swelling. Figure 8.25 shows swelling in annealed and

Fig. 8.24. Variation of the function F(η ) in Eq. (8.124) with temperature, illustrating the shift of the peak with dose rate, K0 . Parameters used to construct the curves are as follows: ρd = 109 cm−2 , Efv = 1.6 eV, zi − zv = 0.01, zv = 1, 4π RρV = 10−11 cm−2 , Dv = exp(−1.4 eV/kT ) cm2 s−1 (after [15])

Fig. 8.25. (a) Effect of displacement rate on swelling of annealed 316 stainless steel in the RAPSODIE reactor fuel pin cladding at 562 ◦C. (b) Swelling in cold-worked 316 stainless steel in the PHENIX reactor fuel pin cladding at 590 – 610 ◦C (after [25] and [26])

388

8 Irradiation-Induced Voids and Bubbles

cold-worked 316 stainless steel at temperatures between 562 and 610 ◦C over a range of dose rates. Note that increasing dose rate has the effect of reducing the swelling rate at a given dose, but that at steady state, all data have a similar slope, indicating that the primary effect of dose rate is on the duration of the swelling transition period. If we move up the temperature scale, we can restore the same relative ratio of recombination rate to absorption rate at sinks. In fact, by requiring that this ratio be invariant, we can obtain a relationship between temperature and dose rate, termed the temperature shift. 8.3.5 Irradiation Variable Shifts The concept of variable shifts was developed to provide a better understanding of the relationship between variables in swelling [16]. The idea is that when one irradiation variable is changed, a shift in other variables can be determined that will preserve a physical quantity describing the behavior of defects during irradiation. There are two such quantities that pertain to the limiting case where recombination dominates defect loss. The number of defects per unit volume that have recombined up to a time τ is: NR = Kiv

τ 0

CiCv dt .

(8.151)

When the solid is at steady state and defect concentrations are controlled by recombination, Eq. (8.116) give:

K0 zi Di 1/2 Kiv zv Dv K0 zv Dv 1/2 Ci = , Kiv zi Di Cv =

(8.152)

and substituting into Eq. (8.151) yields: NR = K0 τ .

(8.153)

The number of defects lost to sinks per unit volume up to a time τ is: NSj =

τ 0

K jC j dt ,

(8.154)

where the subscript j denotes the defect type. Substituting Eq. (8.152) into Eq. (8.154) gives for vacancies: NSv =

KV (K0 Kiv )1/2

zi Di zv Dv

1/2

Φ,

where Φ is the dose, and the expression for interstitials is identical.

(8.155)

8.3 Void Growth Equation

389

These definitions can be used to determine relationships between any two of the three variables: temperature, dose and dose rate, taking the third to be constant. For example, in the steady state recombination-dominated regime, we may require Ns to be equal for dose 1 and dose rate 1 to that for dose 2 and dose rate 2 at a fixed temperature: KV (K01 Kiv )1/2

zi Di zv Dv

1/2

KV Φ1 = (K02 Kiv )1/2

zi Di zv Dv

1/2

Φ2 ,

and canceling terms in the equality gives:

Φ2 = Φ1

K01 K02

1/2 .

(8.156)

For a given change in dose rate, the shift in temperature required at constant dose to keep Ns invariant is determined by equating the same terms, but with fixed dose, resulting in:

Dv K0

1/2

=

1

Dv K0

1/2 ,

(8.157)

2

v /kT ): or substituting in for Dv from Eq. (4.54), Dv = D0 exp(−Em K02 kT12 ln v Em K 01 . T2 − T1 = K02 kT1 1 − v ln Em K01

(8.158)

For a change in dose, the shift in temperature required to maintain Ns invariant at fixed dose rate is: 1/2

1/2

(Dv Φ )1 = (Dv Φ )2 , and substituting in for Dv :

v E Φ2 1 1 = exp m − , Φ1 2k T2 T1

(8.159)

(8.160)

and re-arranging gives: −2kT12 Φ2 ln v Em Φ1 T2 − T1 = . 2kT1 Φ2 1 + v ln Em Φ1

(8.161)

There is another important temperature shift that, instead of requiring that Ns be invariant, requires the net flux of vacancies over interstitials to a particular type

390

8 Irradiation-Induced Voids and Bubbles

of sink (voids in this case) to be invariant, where the net flux is relevant to void swelling. The temperature shift derived in this way for the recombination-dominated regime to keep swelling rate (NR ) invariant is [16]: kT12 v Em + 2Efv

K02 K01 T2 − T1 = . K02 kT1 1− v ln Em + 2Efv K01 ln

(8.162)

where Efv is the vacancy formation energy. The various variable shifts described in this section are shown in the following figures. Figure 8.26 shows the relationship between dose vs. dose rate dependence at a reference temperature of 200 ◦C for the case of Ns invariant, Eq. (8.156). Figure 8.27 shows the temperature shift as a function of dose rate at constant dose for three values of vacancy migration energy for Ns invariant, Eq. (8.158), and Fig. 8.28 shows the same relationship for the constant dose rate case, Eq. (8.161). Figure 8.29 shows the temperature shift as a function of dose for constant dose rate to keep the swelling rate, NR invariant, Eq. (8.162). Figure 8.30 shows that the temperature shift concept works well in describing the shift in the peak in the swelling vs. temperature curve in nickel over more than five orders of magnitude in the dose rate as given by Eq. (8.162).

Fig. 8.26. Number of interstitials absorbed at sinks as a function of dose at 200 ◦C for different dose rates (after [27])

8.3 Void Growth Equation

391

Fig. 8.27. Temperature shift from the reference 200 ◦C required at constant dose in order to maintain the same point defect absorption at sinks as a function of dose rate, normalized to initial dose rate. Results are shown for three different vacancy migration energies (after [8.27])

Fig. 8.28. Temperature shift from the reference 200 ◦C required at constant dose rate in order to maintain the same point defect absorption at sinks as a function of dose, normalized to initial dose. Results are shown for three different vacancy migration energies (after [8.27])

392

8 Irradiation-Induced Voids and Bubbles

Fig. 8.29. Temperature shift from the reference 200 ◦C required at constant dose in order to maintain swelling invariance as a function of dose rate, normalized to initial dose rate. Results are shown for three different vacancy migration energies and a formation energy of 1.5 eV

Fig. 8.30. Temperature shift of peak swelling as a function of dose rate. Points are experimental data and the line is from theory (after [5])

8.3 Void Growth Equation

393

8.3.6 Stress Dependence Equation (8.125) shows that the void growth rate consists of two components. R˙ th is the thermal emission terms and hence is the only part affected by the state of stress or internal gas pressure. Consequently, the internal gas pressure and stress begin to affect the growth rate only when R˙ th becomes significant, i.e., for temperatures greater than the peak swelling temperature. When the solid is under a hydrostatic stress and when voids contain gas that exerts a pressure on the void surface, the equilibrium vacancy concentration at voids and dislocations will be different from that in the stress-free, gas-free state. Brailsford and Bullough showed that the pressure, but not the external stress, will affect the concentration of vacancies in equilibrium with the void. Hence, the force balance for the void surface of a bubble in mechanical equilibrium, Eq. (8.82), becomes: 2γ , (8.163) R where σ is the hydrostatic stress and p is the gas pressure in the void. (In the case of a non-equilibrium bubble, the appropriate stress is the radial component of the stress tensor, σr .) The vacancy concentration at the surface of the void, given by Eq. (8.85) in the gas-free case, becomes:

Ω 2γ V 0 Cv = Cv exp − p− . (8.164) kT R

σ = p−

Similarly, the equilibrium vacancy concentration adjacent to the network dislocations becomes:

σΩ CvN = Cv0 exp − . (8.165) kT Repeating the solution to the void growth equation using the equilibrium vacancy concentration at the void surface given by Eq. (8.164) and the equilibrium vacancy concentration at the network dislocations given by Eq. (8.165) revises the thermal emission term, Rth in Eq. (8.135) (with ρCP = ρL = 0) as follows: 2γ 0 2 DvCv Ω zv ρd σ + p − R R˙ th = . (8.166) RkT (zv ρd + 4π RρV) Note that shrinkage due to thermal emission becomes instead, stress-enhanced growth when the sum of the external stress and gas pressure exceed the stress due to surface tension: 2γ . (8.167) σ+p> R Note that for a stressed solid containing no gas, stress-enhanced growth will occur 2γ when σ > . For a void containing x gas atoms, Eq. (8.167) becomes: R 3xkT 2γ − σ= . (8.168) R 4 π R3

394

8 Irradiation-Induced Voids and Bubbles

The void radius at which Rcr =

9xkT 8πγ

dσ = 0 is called the critical void radius and is given by: dR

1/2 ,

(8.169)

and substituting into Eq. (8.165) gives the stress at the critical void size, which is the critical stress for unlimited void growth: 4γ 8πγ 1/2 σcr = . (8.170) 3 9xkT The effect of stress on void growth in steel is given in Fig. 8.31. Note that there is little effect of stress out to high dose when the stress is low. But when stress is increased, the swelling increases rapidly at relatively lower doses. Figure 8.32 also accounts for the presence of helium in the growth of voids under stress. However, this formulation predicts that the void growth rate is proportional to stress, which is counter to the 1%/dpa observations. Also, as shown in Fig. 8.32, the effect of stress is only significant at very high temperatures. Experimental data have since shown that the prime role of stress is on shortening the transient swelling regime, rather than increasing the swelling rate in the steady state regime. Figure 8.33 shows the effect of stress on swelling in modified 316 stainless steel alloys irradiated in the PHENIX reactor. Note that with increasing stress, the swelling rate (slope) approaches a constant value at lower doses. Stress can also affect the stability of void nuclei, which would explain the observation of more rapid nucleation.

Fig. 8.31. Stress-enhanced swelling for various stress levels and temperatures as a function of fluence (after [28])

8.3 Void Growth Equation

395

Fig. 8.32. Temperature dependence of stress-enhanced void growth in steel. The solid curves apply to a dislocation density of 109 cm−2 . And a helium production rate of 10−6 appm/s (after [29]) Fig. 8.33. Effect of stress on swelling of two modified 316 stainless steels irradiated in the form of pressurized tubes in the PHENIX reactor (after [30])

In the development of the nucleation rate of voids, the nucleation current and number density of voids of size n was described by Eqs. (8.18) and (8.19), respectively, for the case of vacancy condensation excluding interstitials: −ΔG0n −ΔG0n Jn = Z β N0 exp , and ρ 0 (n) = N0 exp . kT kT

396

8 Irradiation-Induced Voids and Bubbles

with the free energy of formation of void of size n given by Eq. (8.17): ΔG0n = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 . Accounting for the application of an external hydrostatic stress, σh , gives: ΔG0n (σh ) = −nkT ln Sv + (36πΩ 2)1/3 γ n2/3 − nσhΩ ,

(8.171)

ΔG0n (σh ) = ΔG0n (0) + nσhΩ .

(8.172)

and

Note that the effect of gas pressure, p, in the void can also be accounted for by addition of a term, npΩ . When interstitials are present, the free energy is given by Eq. (8.33): ΔGn

δ G0j βi ( j + 1) + exp , = kT ∑ ln βv ( j) kT j=0 n−1

where δ G0j /kT is the increment in free energy of a void in going from j vacancies to j + 1 vacancies if no interstitials are present. By assuming that stress affects only the free energy barrier (and not the critical nucleus size), and that the stress contribution of the energy per atom is not dependent on the number of atoms in the cluster, then we can approximate the free energy in Eq. (8.33) in a manner similar to that done in Eq. (8.172) [31]: ΔGn (σh ) = ΔGn (0) + nσhΩ .

(8.173)

Then, from Eq. (8.35), the ratio of stressed to unstressed steady state nucleation rates in a homogeneous, co-precipitation environment is: Jn (σh ) exp[−(ΔGn − nσhΩ )/kT ] = . Jn (0) exp[−ΔGn /kT ]

(8.174)

Using Eqs. (8.22) and (8.23) to write the ratio of nucleation currents in terms of the ratio of void number densities in the stressed and unstressed state gives: Jn (σh ) Z (σh )βn (σh )ρn (σh ) Z (σh )βn (σh ) exp[−(ΔGn (σh ))] = = , Jn (0) Z (0)βn (0)ρn (0) Z (0)βn (0) exp[−Δ Gn (0)]

(8.175)

and provided that neither the arrival rate ratio, βn (σh )/βn (0), nor Z is sensitive to the stress level [32], then Eq. (8.175) becomes:

ρn (σh ) ≈ exp(nσn Ω /kT ) . ρn (0)

(8.176)

8.3 Void Growth Equation

397

Fig. 8.34. Variation of the void nucleation rate and the void number density as a function of stress and temperature, as described by Eq. (8.176)

Example 8.1. Effect of stress on void density Assuming an external stress of 100 MPa and a void cluster size of ∼ 15 at a temperature of 450 ◦C, Eq. (8.176) gives an increase in the void number density by a factor of ∼ 6. However, for a stress of 200 MPa, the increase is 34 and for 300 MPa, the factor becomes ∼ 200. Since both stress and temperature appear in the exponent, the factor rises rapidly with an increase in stress and with a decrease in temperature (Fig. 8.34). Referring back to Fig. 8.33, the decreasing time to reach the steady state swelling rate as stress is increased, is explainable by stress-enhanced nucleation, which will be more important at lower temperatures, contrary to the effect of stress on the steady state swelling rate.

8.3.7 Effect of RIS Recall from Chap. 6, Sect. 6.4, that RIS (radiation-induced segregation) of the major elements occurs at sinks, which can include voids. The result is a coated void in which the void develops a shell of composition that is different from that in the matrix. As we have seen, for austenitic stainless steels, the void coating is enriched in nickel and depleted in chromium relative to the matrix. A primary effect of the composition change is a change in diffusion coefficient leading to a change in the void capture efficiency. The capture efficiency for the vacancy in the shell is [16, 33]: zV v (rV ) =

1 + δ /rV , 1 + Dvδ /DSv rV

(8.177)

where δ is the thickness of the shell and DSv is the vacancy diffusion coefficient in the shell. Recall that an expression for the composition dependence of Dv in the shell, DSv was determined in Sect. 6.4 of Chap. 6. Using the expression for the capture efficiency in the void growth equations results in a reduction in void growth if DSv < Dv and DSi ∼ Di . A more important effect of the coating is the elastic interaction between a point defect and a void surrounded with a coating that has different elastic constants than

398

8 Irradiation-Induced Voids and Bubbles

the matrix. The result is a change in capture efficiency of the void for defects. The capture efficiency due to a difference in elastic constants is given as:

rV rV Di,v −1 (r ) = + , (8.178) zV i,v V rc (rc + δ )2 wi,v where rc is the void plus coating radius and the transfer velocity, wi,v is: wi,v =

∗ /kT ) Di,v exp(−Ei,v , a

(8.179)

where a is the lattice parameter and E ∗ is the repulsive interaction energy at its largest positive value. The sign of E ∗ is positive (repulsion) if the matrix of the shell is stiffer than that of the matrix. Since E ∗ is proportional to the square of the point defect relaxation volume, the sink efficiency is much smaller for the interstitial than for the vacancy due to the larger repulsion for the interstitial. So the stiffer shell results in a repulsion that is greater for the interstitial than for the vacancy, making void nucleation and growth more rapid in the case of a coated void (Fig. 8.35). A change in the shear modulus or lattice parameter in the shell can also alter the preference of the void for vacancies and interstitials [34] by creating a barrier to defect diffusion through the shell due to a change in the strain energy. When segregation leads to a shell with a shear modulus or lattice parameter only slightly higher than in the surrounding matrix, the void becomes a highly preferential sink for vacancies and swelling is increased. Conversely, a reduction in the shear modulus and

Fig. 8.35. Capture efficiencies for point defects diffusion to a void and a coated void as a function of void radius, rV . The void prefers interstitials, especially at small void sizes. The preference is reversed for the coated void (after [16])

8.3 Void Growth Equation

399

Fig. 8.36. Capture ratio z0i /z0v for coated voids with a shell thickness of two atomic layers and zero surface stress (after [34])

lattice parameter should result in reduced void swelling. Figure 8.36 shows the effect of the shear modulus (1 − μbulk/μshell ) on the interstitial/vacancy capture ratio. For small voids, a few percent change in the shear modulus can result in orders of magnitude change in the capture ratio. Allen et al. [35] compared the swelling and RIS behavior of a range of alloys with different nickel content. Calculation of the lattice parameter for the void shell composition shows that the swelling behavior can be explained by a decrease in lattice parameter at the void surface (Fig. 8.37). In fact, segregation leads to a smaller lattice parameter with a lower shear modulus, and the softer shell reduces void swelling. 8.3.8 Effect of Production Bias Our formulation of swelling was developed under the assumption that only single vacancies and interstitials contribute to the growth or shrinkage of the void. If we wish to include the effect of interstitial clustering and mobility in the damage cascade in this picture, then the most straightforward way to do this is to return to clustering theory and describe the evolution of the void embryo with consideration of interstitial clusters. Numerical solution to the Fokker–Planck equation will yield the void size distribution as a function of time or dose. (An example of the results of such an analysis was presented in Chap. 7 for interstitial loops.) However, numerical solutions are not of much value in understanding the process and the importance of various parameters in the evolution of the void population. Another approach is to consider the effect of the asymmetric production of vacancies and interstitials (production bias) due to differences in the fractions that agglomerate into clusters and

400

8 Irradiation-Induced Voids and Bubbles

Fig. 8.37. Decrease in swelling as a function of changing lattice parameter. Swelling decreases with decreasing lattice parameter, which is caused by RIS at the void surface (after [35])

differences in the thermal stability and mobility of vacancy and interstitial clusters. So we will consider the case when the interaction of the glissile loops with vacancy and SIA loops is negligibly small, in which case, we can develop an analytical expression for swelling which still captures the effect of clustering [36, 37]. Under cascade conditions where clustering is expected to occur, we modify the vacancy and interstitial steady state point defect balance equations by adding in glissile SIA clusters with the following result: 2 vc 2 (1 − εig)K0eff = DiCi (zi kv2 + zdi ρd ) + Kiv DiCiCv + zic v DvCv kni + zi DiCi knv

(8.180) K0eff

2 vc 2 = DvCv (zv kv2 + zdv ρd ) + Kiv DiCiCv + zic v DvCv kni + zi DiCi knv

(8.181)

εig K0eff /xg

= DgCg kg2 ,

(8.182)

where K0eff = (1 − εT )K0 is the effective Frenkel pair generation rate obtained from the NRT rate by accounting for the fraction of Frenkel pairs, εT , recombining dur2 vc 2 ing cascade cooling, and zic v kni and zi knv are the sink strengths of sessile SIA clusters (ic) and vacancy clusters (vc) for the absorption of vacancies (v) and SIA clusg ters (i), respectivly. The quantity, g refers to glissile clusters, εi is the fraction of SIAs in glissile clusters and xg is the mean cluster size. The term kg2 is the total sink strength for the 1D diffusing SIA clusters:

8.3 Void Growth Equation

kg =

1/2 2 πρ dabs + + π R2 ρ V , 4 l(2Rg − l)

401

(8.183)

where dabs is the effective diameter of dislocations for absorbing glissile SIA cluster, Rg and l are the grain radius and distance from the cluster to the grain boundary, respectively. Under cascade damage conditions that allow for intracascade clustering of SIAs and also cluster removal by 1D diffusion of glissile SIA cluster, the void swelling rate is determined by the fluxes of point defects and glissile SIA clusters to voids. Equation (8.110) then becomes: d(ΔV /V ) = (DvCv zv − DiCi zi )kv2 − DgCg xg kg π R2 ρV . (8.184) dt The second term in Eq. (8.184) comes from Eq. (8.182). Under cascade damage conditions, the difference in the point defect fluxes to dislocations due to dislocation bias as well as the recombination and effect of cluster terms in Eqs. (8.180) and (8.181) cause only small perturbations in the swelling rate at steady state. Neglecting recombination and defect cluster terms in Eqs. (8.180) and (8.181), then Eq. (8.184) becomes:

zv kv2 π R2 ρ V d(ΔV /V ) g eff = K0 εi − dt zv kv2 + zdv ρd kg 2 d zv kv zv ρd g +(1 − εi )pl , (8.185) (zi kv2 + zdi ρd )(zv kv2 + zdv ρd ) where pl = (zdi /zdv − zi /zv ) ≈ (zdi /zdv − 1), and zv + zi = 1. The swelling rate is proportional to the effective generation rate and the damage efficiency. The first term in square brackets in Eq. (8.185) is the contribution of the production bias to swelling and is proportional to the glissile cluster fraction explicitly. The second term is due to conventional dislocation bias controlled by single point defects, as is evident by its (1 − εig ) proportionality. For the limiting case of g single Frenkel pair production, where no clusters are formed, εi = 0, the first term vanishes and the swelling rate is driven by single point defect absorption controlled by dislocation bias. The resulting expression is the same as that given in Eq. (8.122) g (neglecting coherent precipitates). Conversely, when εi is close to 1.0, the conventional dislocation bias contribution is small compared to that due to production bias. When both single SIAs and SIA clusters exhibit 3D diffusion, the swelling rate follows an expression analogous to that determined for the single defect, dislocation bias case, Eq. (8.122); however, an SIA cluster term is now included that is analogous to that for single SIAs and can be written as:

g 2 d (1 − εi )p εig pcl d(ΔV /V ) eff zv kv zv ρd = K0 + , (8.186) dt (zv kv2 + zdv ρd ) zcl kv2 + zdv ρd (zv kv2 + zdv ρd ) where pcl = (zdcl /zdv − zcl /zv ) is the bias factor for SIA clusters. Equation (8.186) results in a positive swelling rate for 3D cluster reaction kinetics for any microstructure, similar that in the single defect, dislocation bias formulation, meaning that saturation of swelling will not occur.

402

8 Irradiation-Induced Voids and Bubbles

A permanently positive swelling rate is not physically plausible as swelling is known to saturate at high doses and high values of swelling. In fact, the general behavior of the solution of the Fokker–Planck equation is a gradual broadening of the size distribution until steady state is reached as cascade damage limits further growth of interstitial clusters. According to Eq. (8.185), the swelling rate decreases with increasing void size because of their increasing efficiency for capturing glissile SIA clusters, and the swelling rate will drop to zero when a maximum void size, Rmax , is reached. Under this condition, and if the void density remains constant, the swelling rate saturates when the swelling reaches some value, (ΔV /V )max . In the case where production bias dominates, the saturation void size and saturation swelling become, from Eq. (8.185): Rmax = π dabs /zdv , (ΔV /V )max =

4π max 3 (R ) ρV . 3

(8.187)

Note that neither Rmax nor (ΔV /V )max depend on cascade parameters εi or εT , and Rmax is even independent of the void number density, ρV . If cluster formation is ignored in Eq. (8.185), then the swelling rate does not vanish. The saturation of swelling is an intrinsic property of production bias under cascade damage conditions. As presented in the description of clusters using the Fokker–Planck formulation (Sect. 7.6), it was noted that the cluster size distribution is broadened by the parameter D and shifted by the parameter F. Thus, with increasing dose, the solution to the Fokker–Planck equation describes the broadening of the void size distribution and the increase in the mean void size of the distribution with dose. This general behavior can be compared with experimental swelling results for Fe–Cr–Ni irradiated at 650 ◦C. Figure 8.38 shows that the mean size of the distribution increases from about 11 nm at 9 dpa to over 50 nm by 80 dpa with a corresponding broadening of the distribution. Since swelling is mainly sensitive to the shift of the mean size of the distribution, linear swelling (ΔV /V α dose) is obtained when the growth rate is large compared to the diffusional broadening, in which case the swelling rate is then given by the drift force alone. g

8.3.9 Void Lattices Voids have also been found to organize themselves in periodic arrays, or lattices in a metal under irradiation. Figure 8.39a shows a void lattice in bcc Nb following irradiation with 8.5 MeV Ta+ to a dose of 300 dpa at 800 ◦C, and Fig. 8.39b shows one in Mo irradiated with 2 MeV N+ ions to a dose of 100 dpa at 870 ◦C. The lattices are much easier to form in bcc metals than in fcc metals, though lattices have been observed in Ni, Al and stainless steel. Void lattices are a form of self-organization that occurs as responses of complex systems to external stimuli. It is believed that self-organization results from the collective interaction between system components under external forces that drive the system far from equilibrium. In irradiated solids, the void patterns are believed to be linked to the collective action of the point defects on the lattice structure.

8.3 Void Growth Equation

403

Fig. 8.38. Experimentally measured void size distribution in a Fe–Cr–Ni alloy irradiated at 650 ◦C (after [36])

A full understanding of the formation of void lattices is still lacking, but the theory is able to account for many of the parametric effects in lattice formation. Kinetic rate theory and the determination of an instability threshold can explain many of the observations to date. In general, ordered defect structures form when the following general conditions are satisfied [39]: 1. Agglomeration of vacancies into clusters during the collisional phase of cascade cooling 2. A bias for dislocations towards preferential absorption of interstitials over vacancies 3. An asymmetry in the production and diffusion of mobile point defects (production bias) 4. Some degree of anisotropy during the evolution of clustered defects. This could either be triggered by diffusional anisotropies of point defects, or by anisotropic elastic interaction between defect clusters during the latter stages of their evolution. The occurrence of void lattice formation under cascade damage conditions (neutron or ion irradiation) and its absence under single Frenkel pair production (electron irradiation) is strong evidence for a key role of the 1D motion of thermally stable SIA clusters directly produced in cascades. In fact, it has been shown that when there is anisotropic transport of self-interstitial atoms by the crowdion mechanism (i.e., transport in which some crystal directions are preferred over others), voids occupying spatial positions that form a regular lattice grow faster, on average, than the randomly distributed voids [40]. However, for the void lattice to

404

8 Irradiation-Induced Voids and Bubbles Fig. 8.39. Void lattice in (a) Nb irradiated with 8.5 MeV Ta+ at 800 ◦C to 300 dpa, and helium bubble lattice in (b) Mo irradiated with 2 MeV N+ ions to a dose of 100 dpa at 870 ◦C (after [39])

form, randomly distributed voids have to disappear. This can occur through stochastic void coarsening. Since void evolution in this case is sensitive to the spatial variations in the void growth rate, even a small fraction of interstitials moving as crowdions can significantly affect the spatial behavior of the void ensemble, resulting in the dissolution of randomly distributed voids with lower growth rates by stochastic fluctuations, and the nucleation and growth of voids forming a regular lattice. 8.3.10 Effect of Microstructure and Composition The alloy microstructure can exert significant effects on void nucleation and growth. Microstructure features such as composition, solute addition and precipitate structure are among the most important in influencing void behavior.

8.3 Void Growth Equation

405

Major Element Composition In simple Fe–Cr–Ni austenitic alloys, swelling drops dramatically with increasing nickel content, reaching a minimum at about 50 at%. Figure 8.40 shows that the swelling dependence of nickel holds for various particle irradiations. The effect of Ni content on swelling is primarily due to the change in incubation dose as shown in Fig. 8.41. In fact, the data in Fig. 8.42 shows that at steady state, the swelling rate is the same over a wide range of nickel content. Chromium content also affects swelling of austenitic alloys. Figure 8.43 shows that increasing chromium over the range 15 to 30% results in greater swelling. Less data is available on the systematic effect of Cr than for Ni, but the available data suggests swelling increases monotonically with Cr content. Swelling is much less of a problem in ferritic alloys, but reaches a maximum with a chromium content of about 15 at%. Figure 8.44 summarizes the effect of Ni and Cr on swelling in Fe–Cr–Ni alloys at 675 ◦C. Solute Additions Void swelling should be inhibited by additions of minor elements that bind either vacancies or interstitials with sufficient strength to reduce the effective mobility, thus preventing defects from reaching sinks and promoting recombination. The effect of solutes on the point defect balance equations was presented in Chap. 6, Sect. 6.4. The effect of solute addition on void swelling behavior can be determined by solving Eq. (6.57) through Eq. (6.61) and the nucleation rate, Eq. (8.35), and the void

Fig. 8.40. The effect of bulk nickel concentration on swelling resulting from irradiation with different particles: neutrons, nickel ions and protons (after [35])

406

8 Irradiation-Induced Voids and Bubbles

Fig. 8.41. The influence of temperature and nickel content on swelling of ternary Fe–15Cr– xNi alloys in EBR-II (after [41])

swelling rate, Eq. (8.112). Results of numerical methods solution [42] show that with increasing values of binding energy, the activation energy for void nucleation increases (Fig. 8.45). The void swelling rate decreases with increasing binding energy as shown in Fig. 8.46. The net effect of solute addition on void swelling is shown in Fig. 8.47 which indicates that for increased solute concentration and binding energy, void swelling decreases. Data on the role of solutes in swelling is in general agreement with the model. Figure 8.48 shows that Si and P strongly influence the swelling of austenitic stainless steels. In fact, Si is a fast diffuser and is known to alter the ratio of diffusivities of the solvent atoms. As shown in Fig. 8.49, the effect of P on swelling is indeed in extending the incubation period to larger doses. Oversize solutes such as Hf have a similar effect in suppressing the nucleation of voids in stainless steels irradiated at ∼ 300 ◦C. While other factors are important, Fig. 8.50 shows that the addition of ∼ 1 wt% Hf to 316 stainless steel results in the suppression of void formation during Ni++ ion irradiation at 500 ◦C through a dose of 50 dpa, compared to an incubation dose of only 2 dpa for the reference 316 stainless steel alloy. Precipitates Precipitates can act as recombination sites for vacancy–interstitial annihilation to reduce void swelling. Precipitates can also inhibit dislocation climb necessary for dislocations to act as a preferential sink for interstitials and hence, retard void growth.

8.3 Void Growth Equation

407

Fig. 8.42. Swelling of Fe–15Cr–Ni ternary alloys in EBR-II at temperatures between 400 and 510 ◦C for nickel levels between 12.1 and 24.4 wt% (after [41])

In fact, precipitates can affect cavity growth in three ways [46]. The first is a direct effect in which voids that are attached to precipitates can undergo large growth rates because the precipitate acts as a collector of point defects. Precipitates can indirectly affect void growth by changing the overall sink strength of the solid, or by changing the characteristics of the matrix. As discussed in Sect. 5.8, the coherent precipitate is considered to be a site where constrained recombination of defects occurs due to the distribution of saturable traps that acquire a steady state occupation probability as a result of a balance between defect capture, defect thermal release and extrinsic recombination with the antidefect. However, incoherent precipitates accept any excess point defect flux that happens to impinge on it. These precipitates can accumulate defects and may act as sites for rapid transport of defects, similar to grain boundaries. In fact, they can serve as sites for the collection of defects which are then channeled to voids.

408

8 Irradiation-Induced Voids and Bubbles

Fig. 8.43. Effect of chromium content on swelling in Fe–Cr–Ni alloys following 5 MeV Ni+ ion irradiations to a dose of 140 dpa (after [19])

Fig. 8.44. Two-dimensional plot of the nickel and chromium dependence of swelling in Fe– Cr–Ni alloys irradiated with 5 MeV Ni+ ions at 675 ◦C to a dose of 140 dpa. Swelling was measured by the step-height technique (after [19])

8.3 Void Growth Equation

409

Fig. 8.45. The effect of impurity trapping on the free energy of void nucleation. Upper curves are for vacancy trapping and lower curves for interstitial trapping. The nucleation rates calculated from the curves are given as a function of binding energy in eV (after [42])

While the potential exists for precipitates to strongly influence void growth through their action as sinks or recombination sites, measurements of the effect of precipitation on void growth have failed to show that they play a significant role. 8.3.11 Effect of Reactor Operating History Much of our understanding of void behavior in metals comes from irradiation in reactors. The experimental data is used to validate models and to provide material parameters to benchmark the models. Given that most models assume that reactor parameters (temperature, dose rate, stress) are constant over time, it is often

410

8 Irradiation-Induced Voids and Bubbles

Fig. 8.46. The effect of impurity trapping on void growth rates. Upper curves are for vacancy trapping and lower curves are for interstitial trapping (after [42])

true that in both commercial and test reactors, these parameters can vary considerably during operation and due to the shutdown-startup cycle. It is not unusual for irradiation experiments to experience numerous power (and hence, temperatures) reductions over the course of a sixth month to one year irradiation. Garner [47] cites one instance in which a 600 ◦C, three-year irradiation experienced 237 temperature setbacks in the first year, during which the temperature fell to as low as 50 ◦C. While the dose accumulated at these lower than target temperatures is low (0.12 dpa in the 3.5 dpa accumulated in year 1), they can have a profound effect on the mi-

8.3 Void Growth Equation

411

Fig. 8.47. The fraction of traps occupied for vacancy trapping at typical charged particle and fast reactor dose rates and temperatures vs. binding energy. Under these conditions, the fraction of traps occupied is small even at high vacancy binding energies (after [42])

crostructure. Figure 8.51a shows the difference of dislocation loop size and number density in Ni–2.0Si samples irradiated in JMTR at 400 ◦C for the case of “conventional” temperature control vs. one where the temperature control was considerably improved. The smaller mean loop size and larger density is likely the result of additional loop nucleation during the periods where temperature was low but the neutron flux was non-zero. This low-temperature microstructure persisted at the nominal irradiation temperature and resulted in an alteration of the loop size distribution as compared to the case in which temperature was controlled. Low-temperature loop nucleation in a high temperature microstructure can also affect the evolution of the void microstructure. Figure 8.51b shows the microstructure of a Fe–15Cr–16Ni alloy irradiated at 600 ◦C in the Materials Open Test Assembly (MOTA) in the Fast Flux Test Facility (FFTF) to comparable doses. The sample on the left was in an assembly, reactor shutdown occurred over a six-hour period during which the temperature was reduced by 50 – 100 ◦C and then to gradually over the six-hour period during which the flux was also decreased. Irradiation during cooling is responsible for the formation of the fine dislocation loop structure. Following rapid shutdown during which the neutron flux and temperature is decreased over a several minute period, no fine loop structure is observed. The fast drop in temperature does not provide an opportunity to accumulate enough dose in this intermediate temperature regime to cause loop nucleation.

412

8 Irradiation-Induced Voids and Bubbles

Fig. 8.48. Influence of (a) silicon and (b) phosphorus on the swelling in EBR-II of annealed Fe–25Ni–15Cr at various combinations of temperature and fluence (after [43])

8.3 Void Growth Equation

413

Fig. 8.49. Influence of phosphorus level on swelling in EBR-II for a titanium-modified 316 steel at 425 and 540 ◦C (after [44])

Fig. 8.50. Suppression of swelling to at least 50 dpa in 316 SS doped with ∼ 1 wt% Hf after irradiation with 5 MeV Ni++ ions at 500 ◦C (after [45])

414

8 Irradiation-Induced Voids and Bubbles

Fig. 8.51. (a) Effect of temperature control on dislocation loop formation and growth in Ni–2%Si irradiated at 400 ◦C in the Japan Materials Test Reactor (JMTR) to a dose of ∼ 1024 n/m2 . LHS is convential control (0.92 ×1024 n/m2 , E > 1, 0 MeV), RHS is improved control (0.96 ×1024 n/m2 ). (b) Effect of shutdown rate on the formation of small dislocation loops in Fe–15Cr–16Ni irradiated at in FFTF at 600 ◦C. The image on the left underwent a slow temperature decrease during power shutdowns compared to a very rapid reduction in temperature at shutdown for the sample on the right (after [47])

The significance of these observations is twofold. First, that a low-temperature dislocation microstructure introduced into a high-temperature microstructure can alter the further development of that microstructure, affecting both loop and void evolution. Second, only very small doses (< 0.1 dpa) are required to nucleate the fine loop structure that remains stable during the continuation of the irradiation at high temperature. This data also provides additional information on the loop nucleation rate, indicating that it is perhaps higher than current models can explain.

8.4 Bubble Growth

415

8.4 Bubble Growth Up to this point, we have been treating voids as essentially empty cavities that grow and shrink by the absorption of vacancies. We have accounted for the effect of gas atoms on the nucleation of voids and also on the equilibrium vacancy concentration at the void surface. But we have not discussed the magnitude of the pressure in the void due to the gas and the effect this may have on the growth of the void. We also have made no distinction between a void and a bubble. One question that we would like to answer is how much gas must a void have in order to be considered a bubble? In a practical sense, the distinction is largely one of degree and character. A cavity is considered to be a bubble if the effect of the gas (on the surface energy and due to the pressure) causes the cavity to become spherical. This is essentially how voids and bubbles are distinguished in transmission electron microscopy. Due to the periodicity of the lattice, cavities will be faceted with the facets lying on the close-packed planes. But if the surface energy is changed by the gas, or if the gas pressure is high enough, then the cavity will become spherical in shape. Of course, very large voids will approach a spherical shape as the contribution of the facets diminishes with increasing void radius. Because insoluble gases are often formed by transmutation when certain elements are irradiated, inert gas bubbles form, which alter the mechanical and physical properties of an alloy. Bubble formation depends on the mobility of the gas (either in the form of individual atoms or complexes), the minimum number of gas atoms which are able to form a stable nucleus and the rate at which lattice vacancies can be supplied to enhance the stability of a nucleated core. Bubbles nucleate under irradiation and then grow or redissolve. The criterion is that nucleation ceases when a gas atom diffusing at random is most likely to encounter a pre-existing nucleus rather than take part in creating a new one. The resulting bubble density varies inversely as the square root of the gas atom diffusion coefficient and thus increases with decreasing temperature. The following assumptions about bubble nucleation under irradiation are made. Homogeneous nucleation is predicated on the premise that bubbles grow by the interaction of gas atoms from a background atomic population on a random basis. Thus, no account is taken of local effects such as cascade processes or precipitation on lattice defects or impurity agglomerates. Concerning stable nuclei, we assume that a pair of gas atoms is stable against thermal dissociation and that its activation energy is such that its motion may be ignored with respect to that of single gas atoms. In this section, we will first consider the mechanics of bubbles followed by the development of bubble growth models that will closely parallel void growth. 8.4.1 Bubble Mechanics For a gas-filled bubble of radius R, embedded in a solid medium, the change in the free energy of the solid due to the bubble is: dG = V dp + γ dA .

(8.188)

416

8 Irradiation-Induced Voids and Bubbles

Since V dp = d(pV ) − p dV ,

(8.189)

and for an ideal gas, pV = constant and V = 4/3π R3, then: dG 2γ = −4π R2 p − . dr R

(8.190)

Setting dG/ dr = 0 yields: p = 2γ /R .

(8.191)

Thus, the equilibrium condition for a bubble is expressed by the force balance p = 2γ /R, in which the force due to the outward pressure of the gas, p, is balanced by the inward-acting force due to the surface tension, 2γ /R. In the presence of a stress, the force balance becomes: 2γ −σ . (8.192) p= R where positive stress is tension. All bubble models require a specific relation between the number of gas atoms in a bubble and its radius. The van der Waals equation of state is used to describe the thermodynamic state of inert gas in bubbles. Letting nx be the number of gas atoms in a spherical bubble of radius R and the gas density is ρg . Then: nx = (4/3π R3)ρg .

(8.193)

From the idea gas law (pV = nkT ), we have: p

V = kT n

or

p = kT ρg

or

p=

3nkT . 4 π R3

(8.194)

Using Eq. (8.191) for mechanical equilibrium to eliminate ρg and p in Eqs. (8.193) and (8.194) gives: nx = 4/3π R3

2γ RkT

(8.195) 8 π R2 γ . 3kT For small R, 1/ρg is not proportional to R and we must account for the volume occupied by the gas atoms themselves. We do this by modifying Eq. (8.194) to include a term B which is a function of temperature and pressure. This gives us van der Waals equation of state: kT 1 1 − B = kT or = B+ P R, (8.196) ρg ρg 2γ =

and Eq. (8.195) becomes: nx =

4/3π R3 8 π R2 γ = . 3(kT + 2Bγ /R) B + (kT /2γ )R

(8.197)

8.4 Bubble Growth

417

For large R, the perfect gas approximation applies, and for very small R, the dense gas limit applies. Physically, there is a minimum volume occupied by each atom, B and as R decreases, the volume per atom approaches this limit. The result is: nm3 1 : dense gas limit , =B ρg atom and 1 ∼ = ρg

kT 2γ

(8.198)

R : ideal gas limit .

(8.199)

Note that for stainless steel at 500 ◦C, where γ ∼ 1.75 J/m2, 2γ /kT ∼ 328 nm−2 and 1 ∼ nm3 . = 3 × 10−4R ρg atom The limiting cases corresponding to Eqs. (8.198) and (8.199) are: 4 π R3 nx = for small R (8.200) 3B 2γ 4 π R2 for large R . (8.201) = 3 kT If Eq. (8.191) is not satisfied, then the bubble is described as a non-equilibrium bubble. That is, the bubble is not in equilibrium with the solid. Mechanical equilibrium is usually maintained by a flow of vacancies to the bubble to provide the additional volume needed to accommodate the influx of gas atoms. Whether Eq. (8.191) is satisfied depends on the relative absorption rates of vacancies and gas atoms by the bubble. A bubble of radius R can be considered as the absence of (4/3π R3)/Ω matrix atoms where Ω is the atomic volume. The empty sphere of radius R can be thought of as consisting of nv vacancies given by: nv =

4/3π R3 . Ω

(8.202)

The number of gas atoms in a sphere of radius R in mechanical equilibrium is given by Eq. (8.197). The number of vacancies per gas atom in an equilibrium bubble is then: kT R nv B = + . (8.203) nx 2γ Ω Ω Note that nx increases as R2 but nv increases as R3 , so increasing numbers of vacancies are needed per gas atom in order to maintain equilibrium. Stress is accounted for by taking Eq. (8.192) and substituting in from Eq. (8.194) for p gives:

σ=

2γ 3nx kT − , R 4 π R3

(8.204)

418

8 Irradiation-Induced Voids and Bubbles

where σ is the hydrostatic tensile stress. The critical bubble radius for unstable bubble growth is determined by setting dσ / dr = 0 and solving for R, yielding: Rc =

9nx kT 8πγ

1/2 .

(8.205)

Substituting for Rc in Eq. (8.205) into Eq. (8.204) gives:

σc =

128πγ 3 81nx kT

1/2 ,

or nx =

128πγ 3 . 81σc2 kT

(8.206)

The critical bubble radius, Rc is related to the equilibrium bubble radius, R0 by expressing Eqs. (8.201) and (8.205) in terms of the number of gas atoms in the bubble, nx and eliminating nx , giving: √ Rc = 3R0 , (8.207) and the critical stress in terms of R0 is: √ 4 3γ σc = . 9R0

(8.208)

Substituting for Eq. (8.201) into Eq. (8.204) to eliminate nx gives a relation between the applied stress, the initial bubble size and the critical bubble size: R20 2γ σc = 1− 2 . (8.209) Rc Rc Equations (8.208) and (8.209) provide the bubble stability criterion in terms of the applied stress and the bubble size. For bubbles of size R0 , Eq. (8.208) gives the critical stress for stability. For a solid with bubbles of size R0 < Rc , application of a tensile stress σc will cause the bubble to grow to size Rc specified by Eq. (8.209). If R0 > R or if σc is greater than the right hand side of Eq. (8.208), then the bubble will grow without bound. Or, for a given applied stress, Eq. (8.208) gives the critical bubble radius for stability. Equation (8.205) can be compared to the stability equation for a gas-free void in a solid subject to a stress, σ . For p = 0 in Eq. (8.192), we have that σ = 2γ /R. The numerical coefficient in Eq. (8.208) is about 0.77, which is less by about a factor of 3 than the coefficient for the void. The difference is due to the effect of the gas pressure in the bubble that assists the stress. 8.4.2 Growth Law Analogous to void growth, the time rate of change of the volume of a bubble is equal to the difference in the rates at which vacancies and interstitials are absorbed and to the volume carried by each of these point defects: d 4 3 π R = Ω 4π RDv Cv − CvV − 4π RDi Ci − CiV , (8.210) dt 3

8.4 Bubble Growth

419

and so the growth law is: dR Ω ≡ R˙ = Dv Cv − CvV − Di Ci − CiV , dt R

(8.211)

where CvV and CiV are the concentrations of vacancies and interstitials at the bubble surface and Cv and Ci are the point defect concentrations in the bulk solid. The thermodynamic vacancy concentration at the bubble surface given by Eq. (8.85) is modified to include the effect of gas pressure in the bubble:

−Ω 2γ CvV = Cv0 exp p− , (8.212) kT R and for interstitials

Ω 2γ V 0 Ci = Ci exp p− , kT R

(8.213)

where Cv0 and Ci0 are the thermodynamic equilibrium concentrations of vacancies and interstitials respectively for a stress-free solid and the exponential terms reflect the presence of a mechanical stress acting on the solid equal in magnitude to p − 2γ /R. Because Ci0 is so small, the interstitial term, Eq. (8.213) can be neglected. Setting dR/ dt = 0 in Eq. (8.211) and substituting Eq. (8.212) for CvV into the resulting expression, taking logarithms and re-arranging gives [48, 49]: Rc =

2γ , kT p+ ln Sv Ω

(8.214)

where Sv is the effective vacancy supersaturation given by: Sv =

DvCv − DiCi . DvCv0

(8.215)

Now, substituting Eq. (8.194) for p into Eq. (8.214) and re-arranging gives: g(Rc ) = R3c −

2γΩ 2 3nx Ω Rc + =0, kT ln Sv 4π ln Sv

(8.216)

where the expression is denoted by the function g(Rc ), which is zero when Rc is a root. The growth rate is plotted as a function of void radius in Fig. 8.52 for three conditions. The lower curve is the case where Eq. (8.216) has three real roots, the middle curve shows the case in which at least two of the roots are equal and the upper curve has one real root [49]. In case I, the roots are denoted RBc and RV c . A void B containing enough gas atoms that it is between RBc and RV c will shrink back to Rc . B A void with the same number of gas atoms but with radius below Rc will grow to RBc and stop. Finally, a void with the same number of gas atoms and with radius above RV c will grow without limit by bias-driven growth. As the number of gas atoms increases, Eq. (8.216) is represented by curves that progress from I to II to III. In

420

8 Irradiation-Induced Voids and Bubbles Fig. 8.52. Schematic plot of cavity growth rate as a function of cavity radius for increasing amount of helium gas in the void or Sv (after [48])

the case of curve III, the number of gas atoms is large enough that there will be no intersections with the dR/ dt = 0 axis and these cavities will only grow by biasdriven growth. At some critical number of gas atoms, there is just one intersection of the function dR/ dt with the dR/ dt = 0 axis. This case is represented by curve II. In this case, the corresponding number of gas atoms is denoted as n∗x and the ∗ corresponding minimum critical radius where RBc and RV c coincide is denoted as Rc . ∗ The quantity, nx is the maximum number of gas atoms that may be contained in a cavity for there to still exist a critical radius, with a minimum value of R∗c . The minimum critical radius, R∗c can be found by taking the derivative of Eq. (8.216) with respect to Rc , giving: 4γΩ dg(Rc ) = 3R2c − Rc . dRc kT ln Sv

(8.217)

Setting Eqs. (8.216) and (8.217) to zero simultaneously yields the minimum critical radius: R∗c =

4γΩ , 3kT ln Sv

(8.218)

and from Eq. (8.205): n∗x =

128πγ 3Ω 2 . 81(kT )3 (ln Sv )2

(8.219)

Stoller et al. [49] noted that Eq. (8.219) can be written for non-spherical cavities using a shape factor, FV such that: n∗x =

32FV γ 3 Ω 2 , 27(kT )3 (ln Sv )2

(8.220)

8.4 Bubble Growth

421

where FV = 4π /3 for a spherical void. He also notes that more physically reasonable solutions are obtained using a hard-sphere equation of state rather than the ideal gas law, which tends to overpredict swelling incubation times. It should also be noted that Eqs. (8.219) and (8.206) are the same when σ is replaced with Ω / ln S, indicating that the stability criterion is the same regardless of whether the solid is acted on by an actual stress or an effective stress defined by the irradiation-induced vacancy supersaturation. A bubble is stable for negative vacancy supersaturation and can be stable or metastable for positive vacancy supersaturation depending on the magnitude of the supersaturation, the gas content and the bubble size according to Fig. 8.52. For a constant stress or irradiation-induced vacancy supersaturation, when the stability limit is reached by gas absorption, a bubble starts to grow by vacancy absorption and is transformed into a cavity. Equations (8.218) and (8.205) describe the bubble-to-void conversion criterion. Equation (8.211) can be used to calculate the swelling rate due to bubble swelling by assuming all gas to be in the bubbles, re-solution to be insignificant and the gas to be ideal such that: p=

nx kT , 4/3π R3ρB

(8.221)

where ρB is the total bubble density and nx = xt ˙ is the gas concentration in the solid being produced by transmutation at a rate of x. ˙ The swelling rate due to bubble growth is: d(ΔV /V )/ dt = (4π R2ρB /Ω ) dR/ dt .

(8.222)

8.4.3 Bubble Growth by Dislocation Loop Punching While vacancy diffusion is the prime mechanism contributing to bubble growth on a fine scale, an additional mechanism for bubble growth in the case of high gas pressure is dislocation loop punching. If the pressure in the bubble is large enough, the stress in the solid nearby may reach a level where dislocation sources can be activated, resulting in the growth of the bubble by punching out a dislocation loop (Fig. 8.53). Recall that the stress required to operate a Frank–Read source is ∼ μ b/l, where l is the spacing between pinning points. Dislocation sources that are easiest to activate will be those with l ∼ r0 , where r0 is the radius of the bubble. So the excess pressure required for the bubble to generate dislocations is then ∼ μ b/r0 . The magnitude of the excess pressure required to generate prismatic dislocations can be determined by comparing the free energy change of the bubble upon creation of a dislocation loop of size equal to the bubble, to the energy of the loop itself [51]. The work to increase the bubble size is: 2γ π r02 b , (8.223) ΔF = −p dV = − p − r0 where p is the pressure in the bubble, V is the bubble volume, γ is the surface energy and b is the Burgers vector. Neglecting the stacking fault energy contribution, the

422

8 Irradiation-Induced Voids and Bubbles

Fig. 8.53. Schematic illustration of the growth of a bubble by dislocation loop punching (after [50])

energy of the prismatic dislocation loop of radius r0 given by Eq. (7.64) is approximated as: EL =

4r0 μ b2 r0 ln , 2(1 − ν ) rc

(8.224)

so that for dislocation loop formation to be energetically possible: p−

2γ r

π r02 b >

4r0 μ b2 r0 ln , 2(1 − ν ) rc

(8.225)

or approximating EL as π μ b2 r0 : p > (2γ + μ b)/r0 .

(8.226)

For typical values of γ and μ , the gas pressure in the bubble must be about an order of magnitude greater that 2γ /r0 before dislocations can be generated and allow the bubble to expand. 8.4.4 Bubble Lattices Similar to void lattices described earlier, high levels of He can result in the organization of gas bubble lattices. In fact, gas bubble lattice formation has been observed in bcc, fcc and hcp metals following He injection at temperatures < 0.3Tm [52]. Helium bubbles in Cu are aligned with dense-packed rows parallel to matrix {111} directions. Johnson et al. [52] measured the lattice constant of the He bubble superlattice in Cu to be aHe = 7.6 nm, corresponding to a bubble density of 1025 bubbles/m3 . Figure 8.54 shows a bright field transmission electron micrograph of a helium gas bubble lattice in molybdenum following 40 keV He+ irradiation to a dose of 5 ×1021 He+ /m2 at 500 ◦C. While the same forces driving the formation of void lattices is expected to apply to bubble lattices, additional interactions may arise due to the close spacing of overpressurized bubbles, such as bubble growth by dislocation loop punching.

Nomenclature

423

Fig. 8.54. He gas bubble superlattice formed in molybdenum following 40 keV He+ irradiation to a dose of 5 ×1021 He+ /m2 at 500 ◦C (after [39])

8.4.5 Helium Production An important ingredient in bubble formation and growth is the production of helium. In a reactor, He production is governed by the boron and nickel contents of the alloy through the reactions: 10

B(n, α )7 Li ,

(8.227)

and the two-step reaction: 58

Ni(n, γ )59 Ni(n, α )56 Fe .

(8.228)

The thermal neutron (n, α ) cross section for 10 B is very large, about 3837b, while the cross section for 59 Ni is for fast neutrons and is only about 4.3b. For thermal reactors then, a large amount of helium is produced early in life from transmutation of boron, but this source burns out by about 1 dpa (∼ 1021 n/cm2). The presence of nickel in stainless steels provides a smaller but sustained source of helium at higher dose. In this regard, thermal reactors produce greater amounts of helium at low dose and in a lower dose rate environment, making low dose helium-induced swelling a greater problem in a thermal reactor than in a fast reactor. Figure 8.55 shows the production rate of helium from an alloy containing 58 Ni and 10 B in the HFIR (thermal) reactor. Note that the production rate of helium is dominated at low fluence by the contribution from 10 B, and at higher fluence by 58 Ni. Helium buildup for the same alloy in a fast reactor and a fusion reactor are shown for comparison. Note that the helium buildup in a fusion reactor matches that in HFIR, and both are higher than that in a fast reactor.

424

8 Irradiation-Induced Voids and Bubbles Fig. 8.55. Helium buildup vs. fluence for stainless steel in HFIR (thermal reactor), a fusion reactor spectrum and a fast reactor spectrum. In the figure, r is the atom fraction of boron or nickel in the alloy and q is the initial fraction of the isotope listed in the figure (after [27])

Nomenclature a AXv,i B Cj C0j CvL dabs d c,e Dj Dc De Ds E Ebj Efj Emj FV g(Rc ) G G0 ΔG ΔG0n ΔGn H J k

Lattice constant Absorption rate of vacancies, interstitials by sink X Volume occupied by a gas atom in a lattice Concentration of species j Thermal equilibrium concentration of species j Vacancy concentration in equilibrium with a dislocation loop Effective diameter of dislocations for absorbing glissile SIA clusters Strength of diffusive spread for clusters (c) or for vacancy emission (e) relative to single point defects Diffusion coefficient of species j Diffusive spread due to cascades Diffusive spread due to vacancy emission Diffusive spread due to single defect jumps Energy Binding energy of specie j Formation energy of specie j Migration energy of specie j Shape factor (= 4π /3 for spherical void) Void growth rate factor, defined in Eq. (8.216) Free energy Free energy of perfect lattice Change in free energy Activation barrier for void nucleation without interstitials Activation barrier for void nucleation with interstitials Enthalpy, also Henry’s law constant Eq. (8.57) Nucleation current Boltzmann’s constant

Nomenclature

kg2 kX2 k2j Kcleff Kj Kiv K eff j K0 K0eff Kxc l Lj mi M Mx n ncr nk , nk nv,i Nd j N0 NR NS p pcl pl Pm Q r r0 R Rg Rc Rcr Riv Rmax R0 R˙ rk , rk S Sj T V

Sink strength for 1D diffusing SIA clusters Sink strength of sink X Total sink strength species j Effective production rate of defects in clusters and free form Loss rate of species j Vacancy–interstitial recombination rate Effective production rate of free defects of type j Defect production rate Effective Frenkel Pair production rate accounting for recombination Rate of gas atom re-solution Distance of cluster to a grain boundary Thermal emission rate of species j Number of interstitial in an interstitial loop Helium concentration Helium cluster of x gas atoms Number of vacancies in a void Number of vacancies in a void of critical size Critical void nucleus cluster size Number of vacancies, interstitials Average number of defects of type j generated in a single cascade Number of lattice sites per unit volume See Eq. (8.151) See Eq. (8.154) Gas pressure Defined in Eq. (8.186) Defined in Eq. (8.185) Probability of nucleating a void embryo of size m Defined in Eq. (8.148) Radius Prismatic dislocation loop radius Void or bubble radius Grain radius Critical bubble radius Critical void radius Vacancy–interstitial recombination rate Saturation void size Equilibrium bubble radius Rate of change of radius, growth rate Critical void nucleus radius Entropy Supersaturation of species j Temperature Volume

425

426

8 Irradiation-Induced Voids and Bubbles

ΔV /V wn x xg zv zi Z Z

Fractional volume Number of ways of removing ρ 0 (n) voids of size n from a solid Number of gas atoms in a void Mean glissile cluster size Vacancy bias factor Interstitial bias factor Zeldovich factor Zeldovich factor in the presence of interstitials or in a stressed solid

αj β βj δ εig εT Φ γ η μ μx ν θ Θ ρ ρx σ τ Ω ξ ζ

Emission rate of species j 2γΩ /kT defined in Eq. (8.71) Absorption rate of species j Thickness of void shell Fraction of interstitials in glissile clusters Fraction of Frenkel pairs that recombines during cascade cooling Fluence or dose Surface energy Defined in Eq. (8.117) Shear modulus Chemical potential of species x Poisson’s ratio Angle between surface and tangent to void, Eq. (8.81) Defined in Eq. (8.98) Void size distribution Density of entity x Hydrostatic stress Time Atomic volume Defined in Eq. (8.15) Defined in Eq. (8.130)

Subscripts B cr CP D g gb hom i j IP L N

Bubbles Critical size Coherent precipitates Total dislocations Glissile clusters or gas Grain boundary Homogeneous Interstitials Defect specie representation Incoherent precipitates Dislocation loops Network dislocations

Problems

s v V 0

427

Sinks Vacancies Void Equilibrium

Superscripts c e L m s V 0

Cascades Vacancy emission Loops Number of vacancies in a void embryo of size m Single defects Voids Equilibrium Minimum critical value In presence of interstitials

∗

Problems 8.1 In a solid where the effect of interstitials are neglected (i.e., where βi /βv = 0), a) Determine the critical void embryo size (in terms of the number of vacancies and void radius). b) Show schematically how the number of vacancies in the critical size void embryo varies with: i) Temperature ii) Degree of vacancy supersaturation iii) Void surface energy iv) The presence of interstitials c) How do your answers to parts (a) and (b) change when an inert gas is present? 8.2 Determine the critical void embryo size for 316 stainless steel (a = 0.3 nm, γ = 1.75 J/m2) irradiated at 500 ◦C so as to produce a vacancy supersaturation of 103 . 8.3 Derive Eq. (8.40). ˙ o for stainless steel (Tm = 8.4 Calculate and plot the relative void growth rate R/R 1823 K) as a function of T /Tm , given that Qvf = 1.4 eV Qvm = 1.09 eV

ρd = 1010 cm−2 Σs = 0.3 cm−1 φ = 1014 n/cm2 s ν = 100 displacements/neutron

428

8 Irradiation-Induced Voids and Bubbles

ziv = 30 Zi = 1.02 Zv = 1.00 a3 = Ω = 0.011 nm3 kT /2γ = 0.01 nm2

ν = 1013 s−1 Neglect voids as sinks (ρV 0) and precipitates (ρCP ∼ 0) and loops as sinks (ρL 0). Assume the vacancy diffusion coefficient is given by Dv = ν a20 exp(−Qvm /kT ) and the equilibrium vacancy concentration is given by Cv = Ω −1 exp(−Qvf /kT ) . Assume the void diameter is 50 nm. 8.5 The equation for growth of a cavity is given by: dR Ω = Dv (Cv − CrV ) − DiCi . dt R Explain what happens to the cavity growth rate if the radiation dose rate doubles. Assume low sink strength and low temperature. Explain what happens if the radiation stops but the sample is held at the same temperature that existed during the radiation. 8.6 A solid is subjected to a neutron flux, resulting in void formation and growth. At time t1 , a condition is reached where the dislocation density is 109 cm−2 , the voids are all 100 nm in diameter at a density of 1014 cm−3 and the void growth rate is zero. In the absence of thermal emission, however, R˙ = 10−2 nm/s. The metal is instantaneously strained such that the dislocation density increases by a factor of 10 and the void growth rate in the absence of thermal emission increases to 8 ×10−2 nm/s. Determine the direction and magnitude of the hydrostatic stress needed to suppress void growth. Assume that the solid contains no dislocation loops or precipitates and that the voids are gas-free. 8.7 Pure nickel has been found to be highly susceptible to void formation when irradiated in a fast neutron spectrum. Along with voids, perfect dislocation loops are found in nickel. In comparison, Fe–18Cr–8Ni stainless steel is less susceptible to void formation and faulted Frank loops are found; but voids are also present. As the nickel content in the stainless steel is increased, two other observations are made. The susceptibility to void formation decreases, and voids that are present are surrounded by a nickel-rich shell.

Problems

429

Given the following information, explain each of these observations.

σ /γ |Ni < σ /γ |Fe , Element σeff (n, α )

RNi < RFe

Cr 0.20

Fe 0.23

Ni 4.20

8.8 a) Explain the reason for the characteristic bell-shaped plot of swelling vs. irradiation temperature. b) How and why is the shape changed by: i) Cold-work prior to irradiation ii) The addition of impurities iii) Grain size c) Explain why swelling and creep can affect each other. 8.9 You are designing the stainless steel fuel cladding for the Advanced Breeder Reactor. Your objective is to delay void nucleation and minimize void growth. Concerning cladding fabrication, you can control: a) Grain size b) Degree of cold-work c) Precipitate density d) Impurity content of the steel. From a design standpoint, you can control the normal operating temperature of the cladding over a window of 100 ◦C. Using void nucleation and growth theory, how can you utilize these five parameters to reach this goal? Be quantitative where possible. 8.10 Annealing is a means of removing radiation damage from an alloy. For stainless steel with both dislocation loop and void populations, explain what will occur when the steel is annealed at 600 ◦C for several hours. In describing the changes during annealing, indicate relative rates and endpoints. 8.11 In the absence of gas atoms, we wish to eliminate voids in Cu by thermal treatment at 400 ◦C. Calculate the length of time needed to accomplish this for an initial void radius of 5 nm and 30 nm. The surface free energy of copper is 1.73 J/m2. 8.12 Given that the number of gas atoms in a bubble can be described as m = (4/3π R3)ρg and that the gas atom density, ρg , can be described by 1/ρg = B + (kT /2γ )R where B is the dense gas limit: a) Show that the volume increase that accompanies coalescence of equal size gas bubbles is given as (ΔV /V )final /(ΔV /V )initial = /2 .

430

8 Irradiation-Induced Voids and Bubbles

b) Assuming that the overall gas balance in UO2 can be given as Y F t = mN where Y = noble gas yield of a fission event F = fission rate density m = gas atoms per bubble N = bubble density, and all the gas remains in bubbles. Develop an expression for the volumetric swelling rate and indicate the dependence on burnup. c) How would you account for i) Gas remaining in the matrix? ii) Re-solution?

References 1. Cauthorne C, Fulton E (1967) Nature 216:575 2. Jenkins ML, Kirk MA (2001) Characterization of Radiation Damage by Transmission Electron Microscopy. Institute of Physics Publishing, Philadelphia, PA 3. Adda U (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 31 4. Olander DR (1976) Fundamental Aspects of Nuclear Reactor Fuel Elements, TID26711-P1. Technical Information Center, USERDA, Washington, DC 5. Mansur LK (1994) J Nucl Mater 216:97–123 6. Russell KC (1971) Acta Met 19:753 7. Powell RW, Russell KC (1972) Rad Eff 12:127 8. Katz JL, Wiedersich H (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 825 9. Russell KC (1979) Acta Met 26:1615 10. Packan NH, Farrell K, Stregler JO (1978) J Nucl Mater 78:143 11. Wiedersich H, Katy JL (1979) Adv Colloid Interface Sci 10:33 12. Russell KC (1972) Acta Met 20:899 13. Katz JL, Wiedersich H (1973) J Nucl Mater 46:41 14. Semenov AA, Woo CH (2002) Phys Rev B 66:024118 15. Brailsford AD, Bullough R (1972) J Nucl Mater 44:121–135 16. Mansur LK (1978) Nucl Technol 40:5–34 17. Brimhall JL, Kissinger HE, Kulcinski GL (1972) In: Corbett JW, Ianiello LC (eds) Proceedings of Radiation-Induced Voids in Metals, CONF-710601, USAEC Technical Information Center, Oak Ridge, TN, 1972, p 338 18. Garner FA, Porollo SI, Vorobjev AN, Konobeev YuV, Dvoriashin AM (1999) In: Ford FP, Bruemmer SM, Was GS (eds) Proceedings of the 9th International Symposium on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, The Minerals, Metals and Materials Society, Warrendale, PA p. 1051 19. Garner FA (1984) Irradiation performance of cladding and structural steels in liquid metal reactors, chap 6. In: Frost BRT (ed) Materials Science and Technology, vol 10A, Nuclear Materials, part I. VCH, New York

References

431

20. Krasnoselov VA, Prokhorov VI, Koleskikov AN, Ostrovskii ZA (1983) Atomnaya Energiya 54(2)111–114 21. Garner FA, Bates JF, Mitchell MA (1992) J Nucl Mater 189:201–209 22. Brager HR, Garner FA (1979) Effects of Radiation on Structural Materials the 9th International Symposium, STP 683. America Society for Testing and Materials, Philadelphia, PA, 1979, pp 207–232 23. Dupouy JM, Lehmann J, Boutard JL (1978) In: Proceedings of the Conference on Reactor Materials Science, vol. 5, Alushta, USSR. Moscow, USSR Government, pp 280–296 24. Busboom HJ, McClelland GC, Bell WL, Appleby WK (1975) Swelling of Types 304 and 316 Stainless Steel Irradiated to 8 × 1022 n/cm2 , General Electric Company Report GEAP-14062. General Electric Co., Sunnyvale, CA 25. Seran LJ, Dupouy JM (1982) In: Effects of Radiation on Materials the 11th International Symposium, STP 782. American Society for Testing and Materials, Philadelphia, PA, 1982, pp 5–16 26. Seran LJ, Dupouy JM (1983) In: Proceedings of the Conference on Dimensional Stability and Mechanical Behavior of Irradiated Metals and Alloys, vol 1, Brighton. British Nuclear Energy Society, London, 1983, pp 22–28 27. Mansur LK (1993) J Nucl Mater 206:306–323 28. Brailsford AD, Bullough R (1973) J Nucl Mater 48:87 29. Brailsford AD, Bullough R (1972) British Rep AERE-TB-542 30. Dubuisson P, Maillard A, Delalande C, Gilbon D, Seran JL (1992) Effects of Radiation on Materials the 15th International Symposium, STP 1125. American Society for Testing and Materials, Philadelphia, PA, 1992, pp 995–1014 31. Brager HR, Garner FA, Guthrie GL (1977) J Nucl Mater 66:301–321 32. Wolfer WG, Foster JP, Garner FA (1972) Nucl Technol 16:55 33. Brailsford AD (1975) J Nucl Mater 56:7 34. Wolfer WG, Mansur LK (1980) J Nucl Mater 91:265 35. Allen TR, Cole JI, Gan J, Was GS, Dropek R, Kenik EA (2005) J Nucl Mater 341:90–100 36. Singh BN, Golubov SI, Trinkaus H, Serra A, Osetsky Y, Baraskev AV (1997) J Nucl Mater 251:107–122 37. Golubov SI, Singh BN, Trinkaus H (2000) J Nucl Mater 276:78–89 38. Abromeit C (1994) J Nucl Mater 216:78–96 39. Ghoniem NM, Walgraef DJ, Zinkle S (2002) Comput Aided Mater Des 8:1–38 40. Woo CH, Frank W (1985) J Nucl Mater 137:7 41. Garner FA (1984) J Nucl Mater 122–123:459–471 42. Mansur LK, Yoo MH (1978) J Nucl Mater 74:228–241 43. Garner FA, Kumar AS (1987) Radiation-Induced Changes in Microstructure the 13th International Symposium, STP 955 (Part 1). American Society for Testing and Materials, Philadelphia, PA, 1987, pp 289–314 44. Garner FA, Brager HR (1985) J Nucl Mater 133–134:511–514 45. Gan J, Simonen EP, Bruemmer SM, Fournier L, Sencer BH, Was GS (2004) J Nucl Mater 325:94–106 46. Brailsford AD, Mansur LK (1981) J Nucl Mater 103–104:1403–1408 47. Garner FA, Sekimura N, Grossbeck ML, Ermi AM, Newkirk JW, Watanabe H, Kiritani M (1993) J Nucl Mater 205:206–218 48. Mansur LK, Coghlan WA (1983) J Nucl Mater 119:1–25 49. Stoller RE, Odette GR (1985) J Nucl Mater 131:118–125 50. Evans JH (1978) J Nucl Mater 76–77:228–234 51. Trinkaus H (1983) Rad Eff 78:189–211 52. Johnson PB, Mazey DJ, Evans JH (1983) Rad Eff 78:147–156

9 Phase Stability Under Irradiation

Irradiation can have profound effects on the formation or dissolution of phases by alteration of the stability of those phases. The most direct way in which irradiation can alter phase stability is by causing local enrichment or depletion of solute such that the solubility limit is crossed. But irradiation can also dissolve phases by recoil dissolution, cause disordering by creating anti-site defects, and lead to nucleation and growth of distinct phases. Under specific conditions, irradiation can also lead to the formation of metastable phases including amorphization. Because the phase structure of an alloy can significantly affect the physical and mechanical properties of the material, understanding how irradiation affects phase stability is of great importance for engineering materials.

9.1 Radiation-Induced Segregation and Radiation-Induced Precipitation Radiation-enhanced diffusion (RED), discussed in Chap. 4, and radiation-induced segregation (RIS), presented in Chap. 6, explain how irradiation can increase the atomic transport of atoms in the alloy, and how the coupling between the vacancy and interstitial fluxes and the solute and solvent atoms can lead to enrichment or depletion of solute atoms at defect sinks such as the free surface, grain boundaries, dislocations, precipitate interfaces, etc. Enrichment or depletion of solute can lead directly to precipitate formation if the local solute concentration exceeds the solubility limit, or precipitate dissolution if the solute content is driven below the solubility limit. Recall that the temperature dependence of RIS is such that at low temperatures, RIS is minimal due to low defect mobility and the high recombination rate of vacancies and interstitials, limiting the number available to annihilate at sinks. At high temperature, the high equilibrium vacancy concentration leads to enhanced recombination and faster back diffusion, limiting the degree of RIS. However, at intermediate temperatures, significant participation of the solute in the defect fluxes results in pronounced segregation at sinks. Figure 9.1 shows how RIS can lead to precipitate formation or dissolution at a sink. Enrichment of a solute at a sink can raise the local concentration (Fig. 9.1a) above the solubility limit (shown as a dashed line in Fig. 9.1b) locally. The excess solute can then precipitate as a second phase. If a second phase is already present, then depletion of the solute (Fig. 9.1c) can lead to dissolution of that phase locally (Fig. 9.1d).

434

9 Phase Stability Under Irradiation

Fig. 9.1. Schematic illustration showing (a) enrichment of solute at a sink and (b) its corresponding elevation above the solubility limit, and (c) depletion of a solute at a sink and (d) its corresponding suppression below the solubility limit

A classic example of radiation-induced precipitate formation and dissolution is described in Sect. 6.1.2 and Fig. 9.2 and Fig. 9.3 for the case of RIS in solid solution Ni–Si and Ni–Al alloys. The consequence of a large amount of solute enrichment at sinks is precipitation of a second phase. In the Ni–Si system, Si is undersized relative to Ni and enriches at sinks during irradiation (Fig. 9.2). RIS causes segregation to levels that are well above the solubility of Si in Ni, resulting in formation of a Ni3 Si, γ precipitate. Ni3 Si precipitates at the surface, grain boundaries and dislocation loops. Conversely, in the case of Ni–Al, Al is oversized with respect to Ni and depletes at sinks under irradiation as shown in Fig. 9.3. The result is the dissolution of existing precipitates at those locations. Since the Ni–Al alloy is an initially homogeneous alloy and the Al content is below the solubility limit for Al, no precipitates are present before irradiation. However, as shown in Fig. 9.3, the region behind the depleted zone is enriched in Al and this amount of enrichment exceeds the solubility level at locations that are displaced from the sink interface, resulting in precipitation of Ni3 Al in a subsurface layer a small distance away from the grain boundary and dislocation loops. Both of these examples are consequences of crossing the solubility line for an element in solution by solute enrichment or depletion due to RIS, and constitute a primary mechanism of phase instability under irradiation.

9.1 Radiation-Induced Segregation

and Radiation-Induced Precipitation

435

Fig. 9.2. Formation of γ -Ni3 Si on defect sinks in a solid solution of Ni–6at% Si alloy showing (a) a surface coating of Ni3 Si, (b) toroidal γ precipitates at dislocation loops and (c) a grain boundary coated with Ni3 Si (from [1])

Fig. 9.3. Formation of γ Ni3 Al away from defect sinks in a solid solution of Ni–12.8 at% Al showing (a) a subsurface layer of γ Ni3 Al, and (b) formation of Ni3 Al away from dislocation loops (from [1])

436

9 Phase Stability Under Irradiation

9.2 Recoil Dissolution Atom displacements created within collision cascades can cause the atoms in a precipitate to be ballistically driven into the surrounding matrix, thus contributing to the dissolution of the precipitate. Nelson, Hudson and Mazey [2] developed a model (NHM) for recoil dissolution of precipitates that will be summarized here. For a displacement rate in the solid of K0 dpa/s, the flux of atoms (atoms per unit area per second) from the precipitate surface can be written as ζ K0 . For a spherical precipitate of radius rp , the dissolution rate expressed as the rate of volume shrinkage is given by: dV = −4π rp2 ζ K0 Ω , (9.1) dt where Ω is the atomic volume. Dissolution by recoil re-solution of the solute is balanced by growth of the precipitate due to diffusion of the solute atoms to the precipitate. Even though the solute is being re-distributed between the precipitate and the matrix, the total concentration of solute, C is fixed, and can be expressed as: C = 4/3π rp3ρ Cp + Cs ,

(9.2)

where ρ is the precipitate density and Cp is the concentration of solute in the precipitates and Cs is the concentration of solute in solution. The growth rate of precipitates due to the solute flux is given by: 3DCs rp dV = , dt Cp

(9.3)

where D is the solute diffusion coefficient. The net growth rate of the precipitate is then the sum of terms due to recoil dissolution, Eq. (9.1) and precipitate growth due to diffusion of solute from solution, Eq. (9.3) and can be written as: 3DCs rp dV = −4π rp2 ζ K0 Ω + . dt Cp

(9.4)

Substituting for Cs from Eq. (9.2) gives: 3DCrp dV = −4π rp2 ζ K0 Ω + − 4π rp4Dρ , dt Cp

(9.5)

and writing Eq. (9.5) as a radial growth law gives: drp 3DC − rp2 Dρ . = −ζ K0 Ω + dt 4π rpCp

(9.6)

Equation (9.6) is plotted in Fig. 9.4 and shows that for small precipitate sizes, the growth rate is positive, but at larger sizes where the surface area becomes large, precipitates will dissolve. At the size dictated by zero growth rate, dissolution is balanced by re-precipitation. Note that the effect of irradiation is to result in a type

9.2 Recoil Dissolution

437

Fig. 9.4. Growth rates for precipitates undergoing irradiationinduced dissolution (from [2])

of inverse coarsening in which smaller particles are more stable than larger ones, which is opposite that which occurs by Ostwald ripening. The solute concentration profile can be determined with the use of a cell model in which all precipitates are of the same size and each is in a matrix cell of radius, L with 4/3π L3ρ = 1. In the Wilkes model [3] re-solution deposits the solute atoms homogeneously throughout the cell and constitutes a source term in the steady state solution of the diffusion equation. Figure 9.5 shows the solute source term in the ∂C = D∇2C + ζ K0 , matrix surrounding the precipitate. The diffusion equation is ∂t

Fig. 9.5. Source terms for irradiation-induced re-solution of solute from the precipitate, according to various models. The term rp is the precipitate radius, L is the precipitate spacing, R is the recoil radius in the Frost–Russell model [10, 11], and δ is the shell about rp in the Brailsford model [4]

438

9 Phase Stability Under Irradiation

∂ C = 0 at the cell boundary (r = L), ∂ r r=L and the solute concentration at the precipitate surface equals the equilibrium concentration, C(rp ) = Ce , the concentration is then:

3 ζ K0 rp2 2L (r − rp ) 2 2 C(r) = Ce + − r + rp . (9.7) 2Ω D(L3 − rp3 ) rrp

and subject to the boundary conditions:

The concentration profile of Eq. (9.7) is plotted in Fig. 9.6a and shows that the solute concentration rises from the precipitate boundary, rp and levels out as it approaches the cell boundary, L. The steady state cell boundary concentration, C(L) can be written as an excess concentration: 2DΩ χ= (C(L) − Ce ) ζ K0 (9.8) 2(rp /L) − 3(rp /L)2 + (rp /L)4 , =L 1 − (rp/L)2 and is shown in Fig. 9.6b as a function of precipitate-to-cell radius ratio (r0 /L). Note that for a fixed cell size the cell boundary concentration initially increases since the steady state solute supersaturation is increasing with precipitate surface area. When the precipitate is large, the precipitate surface is close to the cell wall and the back diffusion becomes significant, thus causing a reduction in the concentration. For most practical situations, the volume fraction of precipitate is small so that the precipitate size distribution is to the left of the peak in Fig. 9.6b. As a result, small precipitates will experience a net loss of solute until steady state is reached. An improvement in the treatment of the source term in the simple NHM model is obtained by assuming that particles are spaced infinitely far from each other (dissolution–re-precipitation at one particle is unaffected by others), and that resolution occurs at a uniform rate in a shell of thickness δ around the particle of radius, rp (Fig. 9.5) [4]. For an initial precipitate size of r0 , the resulting size was found to be: 3δ 2 rp (3rp + 2δ ) Θ 3 3 r0 − rp = − , (9.9) 8π Dρp[(rp + δ )3 − rp3 )] 4π rp2 where Θ is the re-solution induced rate of precipitate volume change. The effect of irradiation in this model is to reduce the precipitate size from its original dimension by up to a factor of 2 [3]. Note that for the case where δ → ∞, the result reduces to that given in Eq. (9.6). This result can be compared to the well-known thermal coarsening behavior of precipitates described by Wagner [5] and Lifshitz and Slyosov [6]: r¯p3 − r¯03 =

8DCe γ Vm2 t , 9RT

(9.10)

where r0 is the initial average precipitate radius, Ce is the solubility of the precipitate of infinite radius, Vm is the molar volume, γ is the particle-matrix interface

9.2 Recoil Dissolution

439

Fig. 9.6. (a) Steady state solute concentration in the matrix from Eq. (9.7), and (b) steady state boundary concentration from Eq. (9.8) (from [3])

energy and R is the gas constant. Accounting for irradiation-induced re-solution and irradiation-enhanced diffusion the maximum stable particle size [7, 8, 9] is shown to be: 3aD 1/2 , (9.11) rmax = l f K0

440

9 Phase Stability Under Irradiation

where a is the lattice spacing, l is the linear dimension of the cascade, f is the fraction of solute atoms dissolved and the product l f is the shrinkage by re-solution [2]. When particles are initially larger than the maximum stable size, the maximum size decreases according to: rmax (K0 t) − rmax(K0 t0 ) = −l f K0 (t − t0 ) ,

(9.12a)

and when the initial particle sizes are much smaller than that given by the equilibrium size distribution, then the particle size increases according to: 3 3 rmax (K0 t) − rmax (K0 t0 ) = 9aD(t − t0 ) .

(9.12b)

Note that Eq. (9.12b) is similar to Eq. (9.10) for thermal coarsening. A modification to the Wilkes’s cell model is to provide a source term for the re-deposited solute that is more realistic than having it deposited uniformly in the cell (Wilkes [3]) or uniformly in a shell (Brailsford [4]). Frost and Russell [10, 11] model the rate of solute re-deposition in the matrix using the rate at which recoils originate in the matrix, which depends on the distance from the precipitate center, r according to: Θ 2 rp − (r − R)2 , (9.13) 4rR where Θ is the re-solution rate per atom and R is the recoil distance (Fig. 9.5). Solving the diffusion equation with the spatially dependent source term, G(r): G(r) =

∂C = D∇2C + G , ∂t gives: Θ 3 r − rp3 − 4R r2 − rp2 48RD 1 1 2 − , −6 rp − R2 (r − rp ) − (3rp − R)(rp + R)3 r rp

(9.14)

C(r) = C0 +

and the maximum concentration is given by: Θ R2 R . Cmax = C0 + 1− 12D 4rp

(9.15)

(9.16)

The maximum solute concentration is proportional to the re-solution rate and weakly dependent on the precipitate size. The inverse coarsening rate of particles that are not of the same size can be determined by calculating the diffusion near each particle [10, 11]. The calculation assumes that the concentration at the edge of its cell is an average matrix concentration, and that there is no net flux to or away from a precipitate of some radius, rm giving: rp 1 drp L Θ R3 = 1− , (9.17) 2 2 dt rm rp (L − rp ) 48

9.2 Recoil Dissolution

441

for which solutions exist depending on the value of rm . Assuming that rp L and the initial precipitate size is r0 , then: rp3 (t) r03 rp2 (t) r02

= 1+

t , τA

for rp rm

and τA =

48r03 , Θ R3

(9.18)

= 1−

t , τB

for rp rm

and τB =

24rm r02 , Θ R3

(9.19)

rp − rm = (r0 − rm ) exp(−t/τC ) ,

for r ∼ = rm

and τC =

3 48rm . Θ R3

(9.20)

Note that the relation between the particle size and time is rp3 α t when the size is below rm and rp2 α t when the size is greater than rm . For all cases, when R, r0 and rm are of the order of 10 nm, t is between 10/Θ and 100/Θ . For the case of fast reactor conditions, Θ ∼ 10−7 dpa/s, so 108 s ≤ t ≤ 109 s, which is equivalent to 3 to 30 years. Since the incubation time varies with r3 , larger precipitates would require even longer for inverse coarsening to occur. Consequently, irradiation-induced inverse coarsening by recoil re-solution is expected only after very long-term exposures. The effect of irradiation on precipitate stability is shown schematically in Fig. 9.7 as a series of illustrations with increasing dose. Prior to irradiation, the precipitate is in equilibrium with the matrix solute concentration, Ce (Fig. 9.7a). Irradiation causes dissolution of the precipitate surface and an increase in the solute content near the interface that begins to diffuse away (Fig. 9.7b). Re-solution is balanced by re-precipitation and results in a steady state concentration profile (Fig. 9.7c). Local supersaturation of solute may lead to the nucleation of new precipitates in the matrix (Fig. 9.7d) or if the precipitates are very widely spaced, the matrix solute may not reach a value that results in steady state and the precipitate will continue to dissolve (Fig. 9.7e). Determining the stability of a phase under irradiation is complicated by the influence of multiple parameters such as the displacement rate, temperature, and sink strength. An estimate for the stability of a precipitate can be obtained by considering two opposing processes, ballistic mixing and radiation-enhanced interdiffusion. This problem was analyzed by Abromeit [13] and the analysis is summarized here. Precipitates are assumed to be dissolved by ballistic mixing at a rate approximated by: Rm = β σD φ ,

(9.21)

where the product of the displacement cross section, σD and the flux, φ is the displacement rate in dpa/s, and β is a factor that links displacement rate to solute loss from the precipitate. Similarly, the rate of formation or growth of a precipitate due to radiation-enhanced diffusion is given by: Rg = α D˜ ,

(9.22)

442

9 Phase Stability Under Irradiation Fig. 9.7. Schematic illustration of radiation-induced precipitate dissolution and precipitation as a function of dose. (a) Unirradiated state, (b) surface dissolution at low dose, (c) steady state, and either (d) nucleation of new precipitates due to local solute supersaturation in the matrix, or (e) continued dissolution of the precipitate due to low precipitate density (from [12])

where α is a constant and D˜ is the interdiffusion coefficient. The solubility limit may be determined by equating the two processes, yielding:

α D˜ = β σD φ .

(9.23)

The steady state point defect balance equations are written as in Chap. 5: K0 − KivCiCv − Dvks2Cv = 0 K0 − KivCiCv − Di ks2Ci = 0 ,

(9.24)

and the variables are as defined in Chap. 5, where Kiv = 4π rv Di /Ω , and ks2 = 4π rsCs /Ω is the sink strength. Note that in this analysis, no distinction is made in the sink strength for vacancies and interstitials. When recombination dominates defect loss: 1/2 1/2 D˜ = AK0 Dv (Ω /4π rv)1/2 ,

(9.25)

9.2 Recoil Dissolution

443

and when defect annihilation at sinks dominates, D˜ is temperature-independent and can be described as: D˜ = AK0 /ks2

(9.26)

and A is a constant describing the transport efficiencies of the atoms via vacancies and interstitials. Eliminating D˜ from Eqs. (9.25) and (9.26) defines the boundary between the regimes where recombination is dominant and where annihilation at sinks is dominant and gives: K0 = ks4 Dv (Ω /4π rv ) .

(9.27)

Equation (9.27) is shown by the plane, P1 in Fig. 9.8 that plots the solubility as a function of damage rate, temperature and sink strength. Given that σd φ = K0 /N the contribution of defect annihilation at sinks to the solubility limit is determined by eliminating D˜ between Eqs. (9.21) and (9.26) and yields the critical sink strength: kc2 = Aα N/β .

(9.28)

Equation (9.28) is shown as the plane, P2 in Fig. 9.8. Finally, according to Eqs. (9.23) and (9.25), a temperature-dependent boundary separates the two-phase from the one-phase regimes and is given as: K0 = (Aα N/β )2 Dv Ω /4π rv ,

(9.29)

Fig. 9.8. Stability diagram for precipitates under irradiation in displacement rate-temperaturesink strength space. The plane P1 separates recombination and annihilation regimes, and precipitates are stable below the plane P3 and to the left of the plane P2 (from [13])

444

9 Phase Stability Under Irradiation

and is shown as plane P3 in Fig. 9.8. Precipitates are stable below P3 and to the left of P2 . The region representing stability of the two-phase structure increases in size with increasing temperature due to increasing diffusivity and with increasing values of the critical sink strength, kc2 . The term β in Eq. (9.21) is approximated by β = β1Vc /Ω , where β1 is a constant and Vc is the volume of the collision cascade and is therefore proportional to the cube of the cascade radius, rc [13]. Re-precipitation of the solute dissolved into the matrix by the cascade is controlled by interdiffusion with the rate constant given by Fick’s law as α = 4α1 /rc2 , where α1 is a constant. Inserting these expressions for α and β into Eqs. (9.28) and (9.29) gives: 3π Aα1Ω N 1 , β1 rc5 Aα1 N 2 3Dv Ω 3 1 . K0 = β1 4π 3 rv rc10 kc2 =

(9.30) (9.31)

Note that both the critical sink strength and the production rate/temperature relationship exhibit a very strong dependence on the cascade size. The model was applied to the case of a Cu–48%Ni–8%Fe alloy irradiated with 300 keV Cu+ ions over a range of temperatures and displacement rates. Figure 9.9 plots the primary recoil rate vs. 1/T with the open symbols denoting irradiation-induced dissolution of the two-phase structure. Note that there is a critical displacement rate for irradiationinduced dissolution that increases with temperature. The line in the graph is the optimal fit of Eq. (9.31) to the data, from which the cascade radius was determined to be ∼ 2.7 nm. In summary, radiation-induced dissolution is a key process affecting the stability of precipitates. Radiation results in re-solution of the precipitate outer surface and

Fig. 9.9. Stability of the two-phase structure in Cu–48%Ni–8%Fe irradiated with 300 keV Cu++ . Filled symbols denote irradiation-induced disordering of the twophase structure and open symbols denote no irradiation effect. The line is the best fit of Eq. (9.31) (from [13])

9.3 Radiation Disordering

445

the evolution of the phase microstructure is then determined by the relative rates of re-solution and re-precipitation. In essence, phase stability is controlled by kinetic processes in the solid. Besides dissolution, precipitate stability is also affected by radiation-induced disordering, described in the next section.

9.3 Radiation Disordering The NHM model described in the last section was originally developed for both recoil dissolution and disordering dissolution. Disordering involves the loss of longrange order due to irradiation. In the case of disordering, displacement is assumed to occur in a shell of thickness, l at the precipitate surface and result in the loss of solute atoms by diffusion to the matrix. It is also assumed that only a fraction, f of these solute atoms actually become dissolved. Defining ξ = l f as the dissolution parameter, then the dissolution rate given in Eq. (9.1) becomes: dV = −4π rp2ξ K0 , dt

(9.32)

and the rate of change of the precipitate size due to disordering dissolution is: dr 3DC = −ξ K0 + − rp2 Dρ , dt 4π rpCp

(9.33)

which is identical to Eq. (9.6) except for the first term. Russell [14] points out that since l ∼ 10 nm, then for f ∼ 1, ξ = l f ∼ 10 nm. Comparing this value to the corresponding term in Eq. (9.6) for recoil dissolution, where ζ Ω ∼ 10−4 nm, shows that the disordering dissolution rate is much higher than that due to recoil dissolution, so disordering dissolution is expected to be a much more effective process. Referring back to Fig. 9.4 shows that the stable precipitate size will be lower for disordering dissolution due to its greater efficiency. Irradiation is known to disorder alloys by the creation of vacancies and interstitials and anti-site defects, in which the atoms are re-located to the complementary site, disrupting the order in the alloy. But disordered alloys will return to their equilibrium state as long as diffusion can occur. In fact, the high concentration of vacancies and interstitials produced by irradiation can enhance the ordering process by radiation-enhanced diffusion. Therefore, irradiation causes two opposing processes to occur: disordering and re-ordering. Liou and Wilkes [15] describe the rate of change of order in an alloy due to irradiation starting from the Bragg–Williams definition of long-range order for a binary alloy with atoms arranged on two sublattices, α and β , where the long-range order parameter is defined as: S=

( fAα − XA ) , (1 − XA )

(9.34)

where fAα is the probability of an A atom being on an α lattice site, and XA is the atomic fraction of A atoms. When S = 1, the alloy is completely ordered and when S = 0, the alloy is completely disordered.

446

9 Phase Stability Under Irradiation

Under irradiation, the rate of ordering can by written as a competition between radiation-induced disordering and thermal re-ordering: dS dS dS = + . (9.35) dt dt irr dt th The disordering rate due to irradiation can be written as: dS = −ε K0 S , dt irr

(9.36)

where ε is the disordering efficiency, or the ratio of replacements to displacements, and is of the order 10–100 under neutron irradiation. The thermal order-disorder transition can be written as a chemical reaction in which A and B atoms on the wrong lattice sites are interchanged so that the A–B pair is on the correct sites: Kc

(A − B)wrong (A − B)correct ,

(9.37)

Kw

where the rate constants, Kc and Kw are given by: Kc = νc exp(−U/kT ) , Kw = νw exp[(−U + VT)/kT ] ,

(9.38a) (9.38b)

where U is the energy barrier for the reaction and the activation energy, VT is the energy reduction when the wrong A–B pair transforms to the correct A–B pair and the νc,w are the frequency factors for the correct and wrong pairs, respectively. The solution of the chemical rate equations gives the following relation for the order parameter in terms of the equilibrium order parameter, Se and the time, t: (1 − S) = coth(kot + y) , (1 − Se)

(9.39)

where y is a constant and ko is the rate constant defined as: v i ko = νvCv exp(−Em0 /kT )(Zα + Zβ − 2) + νiσ Ci exp(−Em0 /kT ) (XA /XB )1/2 × Zβ exp(−V0 /2kT ) , (9.40) 1/2

1/2

where 2νv = (νc νw )v and 3νi = (νc νw )i are the frequency factors for exchange v and E i are the vacancy and interby vacancies and interstitials, respectively, Em0 m0 stitial migration energies for ordering, Zα is the number of α sites that are nearest neighbor to a β site and Zβ is the reverse, where α and β refer to the two sublattices, σ is a parameter accounting for the number of reaction paths and their probabilities and XA and XB are the atom fractions of A and B atoms, respectively. V0 is the activation energy for ordering, V0 = AV , where A is crystal structure dependent (A = 6

9.3 Radiation Disordering

447

for fcc and A = 14 for bcc) and V = VAB − (VAA +VBB)/2, where the VXY terms are the energies of the respective atom pairs. The time derivative of the thermal order parameter can be written as [15]: dS ko (1 − S)2 − (1 − Se)ko . = (9.41) dt th (1 − Se) The steady state solution to Eq. (9.35), where the terms are given in Eqs. (9.36) and (9.41), is: (1 − Se ) 2 2 4ko ε K0 1/2 S = 1 + ε K0 − ε K0 + 4ko2 + . (9.42) 2ko (1 − Se) Liou and Wilkes applied this formalism to the AuCu3 system as a function of temperature and dose rate. Figure 9.10 shows that at any given temperature, the effect of increasing dose rate is a reduction in the order, as expected. Also, for a given dose rate, increasing temperatures results in greater order. Another way of showing the competing effects of irradiation and temperature on the alloy order is given in Fig. 9.11a. Here, the equilibrium value of Se is 1.0, but the alloy is in a state where the order, Sobserved is less than Se . At low temperature, where defect motion is restricted, the effect of irradiation is to disorder the alloy. At high temperature, the effect of irradiation is to increase defect mobility so that the order parameter approaches equilibrium, which lies above the original, incompletely equilibrated state. That is, irradiation assists ordering at high temperatures. This behavior is further illustrated by the example shown in Fig. 9.11b, which is a first-order transition of a solid solution alloy in the disordered α phase to an ordered α phase. Under irradiation, the ordered phase becomes disordered at low temperatures, reverting to

Fig. 9.10. Steady state long-range order parameter for Cu3 Au under irradiation for various dose rates (from [15])

448

9 Phase Stability Under Irradiation Fig. 9.11. (a) Effect of irradiation on the temperature dependence of the order parameter for a phase structure that is not at the equilibrium order, Se . (b) Equilibrium phase diagram showing a first-order phase transformation of the disordered a phase to the ordered α -phase. (c) Modification of the phase diagram by irradiation reflecting the change in order as given in (a). (d) Dependence on the irradiationmodified phase diagram with dose rate (from [3])

the α phase as shown in Fig. 9.11c. Since the degree of disordering is dependent on the dose rate, the shape of the phase fields shown in Fig. 9.11c will change at higher dose rate. The dependence of the phase fields on dose rate is shown schematically in Fig. 9.11d, in which the ordered region continues to shrink with increasing dose rate. The change in the phase diagram caused by irradiation-induced disordering constitutes an irradiation modified phase transition as disordering can change the alloy phase structure. Recall that the ordered state is the arrangement of atoms that

9.3 Radiation Disordering

449

minimizes the free energy of the solid. Consequently, radiation-induced disorder increases the free energy of the solid above the equilibrium value. Hence, under irradiation, a new free energy balance may be achieved between adjacent phases in the alloy. Figure 9.12 shows how the compositions of the α and γ phases determined by the common tangent of free energy curves can be changed when irradiation induces an increase in the free energy of the intermetallic β phase, resulting in a partially disordered phase, β . Note that while the ordered β phase is in equilibrium with the α phase at a composition CA , partial disordering by irradiation raises the free energy of the β phase to β and the concentration of A in equilibrium with α and β phases is now CA . Further irradiation can lead to complete disordering, β phase, such that the phase does not form. Note that order-disorder transformation energies are generally in the range of 0.1 to 0.6 eV/atom [16]. The effect of irradiation on ordering can also be understood with the aid of the thermal spike model of the cascade, discussed in Sects. 3.3 and 10.2.4. Recall that the energy density in the core of the cascade can reach values such that the region resembles a liquid-like structure. Wollenberger [12] determined the time dependence of the temperature in the cascade as a function of the distance from the center of the spike, where temperature is normalized to the disordering temperature, Tc and the result is shown in Fig. 9.13 for nickel. In this figure, rc is the value of the cascade radius at which the temperature just reaches the disordering temperature at any time during the thermal spike, which in this case is 2.6 nm. As such, the temperature of the region inside this radius can be assumed to exceed Tc , resulting in disordering of the center of the cascade. Presumably, in the outer regions of the cascade where the temperature is below Tc but where the vacancy density is high, re-ordering will occur. In fact, when the re-ordered shell of a new cascade overlaps the disordered zone from an old cascade, the remaining disorder will be reduced, causing a reduction in the disordering efficiency per cascade with increasing fluence. The consequence of this overlap process is that the long-range order parameter will not completely vanish, even at high fluences.

Fig. 9.12. Schematic illustration of a phase diagram for an alloy with an ordered intermetallic compound, β showing partial disordering to β , and complete disordering, β due to the increase in free energy caused by irradiation (from [14])

450

9 Phase Stability Under Irradiation

Fig. 9.13. Time dependence of the temperature of a thermal spike for different radial locations within the spike (from [12])

At low temperatures where vacancies are immobile, irradiation-induced disordering can occur very quickly in some systems. For example, the γ phase (L12), NiAl3 , is extremely unstable under irradiation [17], becoming disordered following irradiation with 500 keV Kr at RT to a dose of 2 ×1014 i/cm2 [18]. On the other hand, Fe3 Al (bcc) and FeAl (bcc-B2) undergo only partial disordering after 40 dpa of 2.5 MeV Ni+ irradiation [19]. Hence, factors besides dose play a role in the orderdisorder transformation reaction in alloys.

9.4 Incoherent Precipitate Nucleation Irradiation can induce the formation of precipitates in an alloy. Precipitate growth and nucleation can be expressed as a chemical effect of vacancies and interstitials due to high levels of solute supersaturation under irradiation. The supersaturation provides the driving force for the reaction. Maydet and Russell [20] developed a model for the growth of spherical, incoherent precipitates under irradiation and that model is described here. The precipitate is characterized by two variables: the number of solute atoms, x and the number of excess vacancies, n, which is the difference in the number of matrix atoms displaced by the precipitate and x. Precipitates with greater atomic volume than the matrix must have n > 0 to relieve the strain energy, and undersized precipitates must have n < 0. The precipitate behavior is described by its movement in a phase space of coordinates n and x, much as was done with dislocation loops and voids in Chaps. 7 and 8. Figure 9.14 shows how the precipitate can move in phase space by capture of solute atoms, βx , vacancies, βv

9.4 Incoherent Precipitate Nucleation

451

Fig. 9.14. Precipitate trajectories in (n, x) phase space showing the processes giving rise to its motion (from [20])

or interstitials, βi , or the emission of solute atoms, αx or vacancies, αv . The particle moves in phase space with a velocity equal to the frequency of addition of solute or defect times the jump distance: x˙ = βx (n, x) − αx (n, x) ,

(9.43)

n˙ = βv (n, x) − αv (n, x) − βi (n, x) .

(9.44)

The β s are determined from concentrations and diffusivities of the defects and solute and the α s are determined as follows. As with void nucleation, there exists an energy barrier to the growth of the precipitate above some size, such that precipitates below this size equilibrate with each other and growth and shrinkage occur at the same rate. That is, the excess number of (n, x − 1)-mer gaining a solute atom to become a (n, x)-mer is balanced by the reverse process. The same holds for the number of (n − 1, x)-mer gaining a vacancy to become a (n, x)-mer. The equilibrium number of (n, x)-mer is then: ΔG0p (n, x) 1 0 , (9.45) ρp (n, x) = exp − Ωm kT where Ωm is the atomic volume of the matrix phase and ΔG0p (n, x) is the free energy of formation of a precipitate from n matrix vacancies and x solute atoms. The balance between (n, x − 1)-mer and (n, x)-mer can be written as:

βv (n − 1, x)ρp0(n − 1, x) = αv (n, x)ρp0 (n, x) ,

(9.46)

βx (n, x − 1)ρp0(n, x − 1) = αx (n, x)ρp0 (n, x) .

(9.47)

452

9 Phase Stability Under Irradiation

Substituting Eq. (9.45) into Eqs. (9.46) and (9.47) and replacing differences in ΔG0p (n, x) by derivatives, gives:

αv (n, x) ≈ βv (n, x) exp

αx (n, x) ≈ βx (n, x) exp

1 ∂ ΔG0p (n, x) kT ∂n 1 ∂ ΔG0p (n, x) kT ∂x

,

(9.48)

,

(9.49)

where βv (n − 1, x) and βx (n, x − 1) in Eqs. (9.46) and (9.47) vary slowly with n and x and have been replaced with their values at (n, x). The free energy change upon formation of a precipitate from a solid solution that contains a supersaturation of solute and vacancies is given as: ΔG0p = −nkT ln Sv + (36πΩ 2)1/3 γ x − xkT ln Sx +

Ω Ex(δ − n/x)2 , 9(1 − ν )

(9.50)

where Sv is the vacancy supersaturation, Sx is the solute supersaturation, Ω is the atomic volume of the precipitate, δ = (Ω − Ωm )/Ωm , γ is the matrix:precipitate surface energy, E is Young’s modulus, ν is Poisson’s ratio, and the remaining variables are as previously defined. The first two terms are the same as in the formation of a void from a supersaturation of vacancies given in Eq. (8.17) in which the first term is due to the vacancy supersaturation and the second term is the contribution of surface energy (with the number of solute atoms substituted for the number of vacancies in the aggregate). The third term reflects the effect of solute supersaturation, analogous to vacancy supersaturation, and the last term accounts for the elastic (volume) strain energy due to either an excess or deficit of vacancies from the stress-free condition (given by δ = n/x). Substituting into Eqs. (9.48) and (9.49) for αv (n, x) and αx (n, x) into Eqs. (9.43) and (9.44) gives: 1 ∂ ΔG0p , (9.51) x˙ = βx (n, x) − αx (n, x) = βx 1 − exp kT ∂ x 1 ∂ ΔG0p βi n˙ = βv (n, x) − αv (n, x) − βi (n, x) = βv 1 − − exp , (9.52) βv kT ∂ n where from Eq. (9.50) the arguments of the exponents are determined to be: 1 ∂ ΔG0p 2Ax−1/3 = − ln Sx + + B(δ 2 − n2/x2 ) , kT ∂ x 3 1 ∂ ΔG0p = − ln Sv − 2B(δ − n/x) , kT ∂ n with A =

ΩE (36πΩ 2 )1/3 γ and B = . kT 9kT (1 − ν )

(9.53) (9.54)

9.4 Incoherent Precipitate Nucleation

453

The behavior of the precipitate in (n, x) space may be described by constructing nodal lines in (n, x) space along which x˙ and n˙ individually are set equal to zero as follows:

βi 1 ln Sv 1 − , for n˙ = 0 , (9.55) n=x δ+ 2B βv

1/2 1 2A ln S n = xδ 1 + − , for x˙ = 0 . (9.56) x 3Bδ 2 x1/3 δ 2 B Figure 9.15 shows that the nodal lines in (n, x) space converge and cross at a critical point, beyond which they diverge. The critical point (n∗ , x∗ ) is found by solving Eqs. (9.55) and (9.56) simultaneously to obtain: 32πγ 3Ω 2 2γΩ , or rp∗ = − 3(Δφ )3 Δφ

β 1 i ln Sv 1 − n ∗ = x∗ δ + , 2B βv x∗ = −

where x∗ and rp∗ are related by x∗ = is given by:

(9.57) (9.58)

4/3π rp2 , and the irradiation-modified free energy Ω

Δφ = −kT ln Sx − δ kT ln[Sv (1 − βi/βv )] −

kT [ln Sv (1 − βi/βv )]2 . 4B

(9.59)

Figure 9.15 is constructed for the case where δ > 0, that is an excess of vacancies relative to solute. Under this condition, the region above the n˙ = 0 line contains an excess of vacancies and has a greater tendency for emission than capture, giving n˙ < 0, or shrinkage. The opposite is true for the x˙ = 0 nodal line in that the vacancy rich precipitate will increase its strain energy by solute emission, causing x˙ < 0 and

Fig. 9.15. Nodal lines, critical points and precipitate trajectories in (n, x) phase space for growth of an oversized, incoherent precipitate under irradiation (from [20])

454

9 Phase Stability Under Irradiation

supporting growth. As shown, particle growth is determined by the quadrants defined by the critical point. Precipitates grow in quadrant 1 and decay in quadrant 3 and behavior in quadrants 2 and 4 depend on the values of the capture terms. Precipitates that are between the nodal lines cannot escape. When with x > x∗ , precipitates will grow and when x < x∗ , they will decay. In general, irradiation will tend to stabilize a precipitate with δ > 0 and destabilize ones with δ < 0. Note that the unstable case of δ < 0 means that Δφ > 0, which can only occur if the first term in Eq. (9.59) is positive since the second term is always negative as long as βi /βv < 1. Physically, this means that since there is a net arrival of vacancies to the precipitate, those precipitates that need the vacancies to grow (e.g., an oversized precipitate, δ > 0) will be stabilized by irradiation. For an undersized precipitate phase (δ < 0) to grow from a slightly supersaturated solid solution without prohibitive strain energy, the particle must emit vacancies into the matrix. In the absence of excess vacancies, this is easily done, as vacancies arrive at and leave the interface at the same rate (in the absence of growth or decay), and there is no trouble in establishing a net flux tout to allow growth. Under irradiation, the vacancy emission rate is not altered, but the arrival rate is increased by several orders of magnitude. It is then almost impossible to achieve a net emission of vacancies. There will instead tend to be a net gain of solute atoms in the face of the slight solute supersaturation. The excess vacancies thus destabilize the undersized precipitate phase. The same arguments may be used to understand stabilization of an oversized precipitate. The potential function given in Eq. (9.59) has some of the properties of a free energy. It predicts whether precipitates of a given size will be stable under irradiation and provides the minimum stable precipitate size. In the absence of excess vacancies due to irradiation, Δφ in Eq. (9.59) becomes Δφ = −kT ln Sx , which is the Gibbs–Thompson equation. The effect of irradiation is to shift the effective free energy curve for the precipitate vertically by the amount δ kT ln[Sv (1 − βi /βv )]. If Δφ < 0, precipitates larger than x∗ will be stable, and if Δφ > 0, all precipitates will decay. Russell shows this schematically in Fig. 9.16. For this alloy, the θ phase is thermally stable and the ψ phase is not. The effect of irradiation is to destabilize the θ phase (δ < 0) and stabilize the ψ phase (δ > 0), by virtue of the sign of δ . Note that the order of stability is reversed by irradiation so that the θ phase would dissolve and the ψ phase would precipitate. The precipitation of the ψ phase under irradiation is an example of irradiation-induced precipitation in an undersaturated solid solution. The nucleation rate of precipitates due to irradiation can also be estimated. The nucleation rate is the number of precipitate nuclei growing past a certain value of x per unit time and volume [22]. At steady state, the nucleation flux is independent of x, and the nucleation rate can be given at an arbitrary value of x as: Jp (x) =

∞

∑

[βx (x)ρp (n, x) − αx (n, x)ρp (n, x + 1)] ,

(9.60)

n=−∞

and the summation converges rapidly for large values of n due to the effect of strain energy. Figure 9.17 shows how the nucleation rate varies with supersaturation of

9.5 Coherent Precipitate Nucleation

455

Fig. 9.16. Schematic phase diagram showing the effect of irradiation on the stability of incoherent precipitates in the case where the precipitate is thermally stable (θ ) and thermally unstable (ψ ) (from [21])

vacancies and solute in the Al–2%Ge system under irradiation. As expected, the nucleation rate increases with both Sx and Sv , but is more sensitive to Sx . Figure 9.17a shows the huge effect of excess vacancies alone on precipitate nucleation. Excess vacancies elevate the nucleation rate from infinitesimal to a high value giving a high precipitate density. Figure 9.17b shows that the effect of excess interstitials is to reduce the nucleation rate somewhat, but by factors small compared to the huge enhancements due to the vacancies. Irradiation is thus a tool for creating phases which otherwise might be impossible to obtain, and also for preventing the formation of phases that are otherwise stable.

9.5 Coherent Precipitate Nucleation The preceding analysis applies for the precipitation of incoherent precipitates from a solid solution due to irradiation. We consider here the precipitation of coherent precipitates due to irradiation. The distinction between these two cases lies in the behavior of point defects at the precipitate surface. As shown in Chap. 8, incoherent precipitates behave like voids in that defects can be absorbed and emitted. However, the coherent precipitate interface acts as a defect trap such that the defect retains its identity. This feature has the result of reducing the problem of determining the energy change due to precipitation from a two-dimensional (n, x) problem to a one-dimensional (x) problem. Cauvin and Martin [23], as summarized by Russell [14] described the pseudo-equilibrium precipitate size distribution under irradi-

456

9 Phase Stability Under Irradiation

Fig. 9.17. (a) Dependence of nucleation rate on solute supersaturation for various vacancy supersaturation levels, based on a solid solution of Ge in Al at 23 ◦C. (b) Effect of interstitial– vacancy arrival rate ratio on the nucleation rate for several solute and vacancy supersaturation levels, based on a solid solution of Ge in Al at 123 ◦C (from [21])

ation, ρ (x) as:

ρ (x) ρ 0 (x) = B(x) , ρ (x + 1) ρ 0 (x + 1)

(9.61)

9.5 Coherent Precipitate Nucleation

457

where ρ 0 (x) is the equilibrium size distribution in the absence of irradiation produced defects and B(x) is defined by: B(x) =

βv (x)[ρv (x) + ρn(x)] + βi (x)[ρi (x) + ρn(x)] , [βv (x) + βi (x)]ρt (x)

(9.62)

where: ρi (x) = number of clusters with trapped interstitials ρv (x) = number of clusters with trapped vacancies ρn (x) = number of clusters with no trapped defects, ρt (x) = ρi (x) + ρv (x) + ρn(x) . The quantity B(x) is the fraction of solute arriving at the precipitate that does not result in defect annihilation. The thermal and irradiation-modified solubilities are related by: Cirr = C0 B(∞). In parallel with the equilibrium free energy, the pseudo-free energy, ΔG (x) is given in terms of the pseudo-equilibrium precipitate size distribution, ρ (x) as: 1 ∂ ΔG ρ (x) = exp . (9.63) ρ (x + 1) kT ∂ x As with an unirradiated solid solution in which a metastable condition exists if G(x) has a maximum in x, then G (x) must have a maximum in x for metastability in the irradiated state. Recalling that ρ 0 (x) = exp(−G0 (x)/kT ), then Eq. (9.61) can be rewritten using Eq. (9.63) as:

∂ G (x) ∂ ΔG0 (x) = + kT ln B(x) , ∂x ∂x

(9.64)

and B(x) has one of two forms depending on the sign of the term, σ defined as:

σ=

(1 − pi/pv ) . (1 − βi/βv )

(9.65)

where pi,v is the probability of a particular trapping site being occupied by an interstitial or a vacancy. For either case, the value of B approaches a constant with increasing values of x, and in similar fashion for large x:

∂ ΔG0 (x) = −kT ln Sx , ∂x

(9.66)

and Eq. (9.64) can be written as:

∂ G (x) = −kT ln Sx + kT ln B(x) . ∂x

(9.67)

Figure 9.18 shows the terms of the expression in Eq. (9.64) for the pseudo-free energy of the solid solution under irradiation for various values of σ . When σ < 0, if −kT ln B(∞) > −kT ln Sx , then the solution will be metastable, as in Fig. 9.18a. If

458

9 Phase Stability Under Irradiation

Fig. 9.18. Schematic illustration of stability altered by defect recombination at the particlematrix interface. (a) σ < 0, 1 root. (b) σ > 0, 1 root. (c) σ > 0, 2 roots (from [23]). (d) Dose rate-temperature dependence of precipitation of Ni3 Si, γ from undersaturated Ni–Si solid solution alloys irradiated with 1 MeV electrons, – Ni–6at%Si, Ni–4at%Si, – Ni–2at%Si. (e) Increase in temperature at which Zn rich clusters, or G.P. zones are stable with increasing irradiation dose rate by 1 MeV electrons over a range of Zn concentration in the Al–Zn phase diagram. Half circles to the right (left) indicate data at high (low) irradiation flux. Full (open) symbols indicated occurrence (absence) of irradiation-induced precipitation. Dashed line is the stability limit in the absence of irradiation (from [24])

∂ G (x) = 0 may have 0, 1 or 2 roots. The solid solution is σ > 0, then the solution to ∂x stable if there are 0 roots. With one root, the solution is metastable (Fig. 9.18b). But in the case of 2 roots (Fig. 9.18c) the solution is metastable below the value x∗∗ , and the precipitate could never grow to large size. Note that in this model, irradiation will always decrease solid solubility.

9.5 Coherent Precipitate Nucleation

459

Table 9.1. Irradiation-induced precipitation in undersaturated binary alloys (from [24]) Alloy

Projectile

Precipitate

Morphology

MgCd AlZn

e− n e− e− Ni+ e−

Mg3 Cd β Zn G.P. zones and β Zn (100) Ag-rich platelets β NiBe β NiBe

NiSi

n Ni+ e− H+

γ γ γ γ

NiGe CuBe

e− e− Cu+ Cu+ H+ H+ N+ e− n e− e− n, ions, e−

γ Ni3 Ge G.P. zones γ Mo γ Pd3 Fe bcc W WRe3 , W-Re unidentified “ changes of composition

– homogeneous precipitation homogeneous precipitation homogeneous precipitation at interstitial dislocation loops homogeneous precipitation and at interstitial dislocation loops at interstitial dislocation loops “ “ coherent, triggered by inhomogenity of defect production at cavities and dislocation lines homogeneous precipitation at cascades at dislocation loops at dislocation loops at dislocation loop s homogeneous precipitation homogeneous precipitation “ –

AlAg NiBe

PdMo PdFe PdW WRe FeV FeCr various ternaries

Ni3 Si Ni3 Si Ni3 Si Ni3 Si

A compilation of precipitates formed in undersaturated solid solutions due to irradiation is shown in Table 9.1. Note that precipitation can occur with many particle types and over large ranges of temperature and dose rate. The relation between these latter two variables is important and is highlighted in Figs. 9.18d,e. Figure 9.18d is constructed from 1 MeV irradiation of several undersaturated Ni–Si solid solution alloys and delineates the region of Ni3 Si, γ precipitation from the solid solution, as shown by the filled circles. Figure 9.18e shows the dose dependence of solubility in Al–Zn. With increasing dose rate, formation of Guinier-Preston (GP) zones (Zn-rich clusters) in Al–Zn occurs at higher temperatures compared to the stability limit in the absence of irradiation (dashed line). Both of these examples show that irradiation of an undersaturated solid solution can lead to precipitation under irradiation at temperatures where the precipitate would not be thermally stable. They also underscore the strong coupling between temperature and dose rate in irradiation-induced precipitation. In summary, irradiation can affect phase stability by numerous processes: solute enrichment or depletion, precipitate re-solution, precipitate disordering, and irradiation-induced nucleation of both incoherent and coherent precipitates. Irra-

460

9 Phase Stability Under Irradiation

diation can also induce the formation of phases that are not stable under equilibrium conditions or metastable phases. Metastable phase formation is discussed in the next section.

9.6 Metastable Phases Since the term metastable implies a phase with a free energy higher than that of the stable phase under the prevailing conditions of temperature and pressure, it is natural to look to thermodynamics to explain their formation under irradiation. Experimental results seem to indicate a strong role of thermodynamics in the tendency to form metastable phases. Intermetallic compounds with small ranges of solubility and complex crystal structures are prime candidates for transformation to a metastable phase [19]. Also, the change in the free energy of the solid due to irradiation-induced defect buildup argues for a thermodynamic explanation [25]. However, not all transformations can be explained on a purely thermodynamic basis as solids under irradiation are generally far from equilibrium. Irradiation can be considered as similar to a quench process in which the atom configurations are essentially determined during the relaxation period following the collision events. At low temperatures, kinetics are restricted and the formation of complex crystalline structures is unlikely. Irradiation will usually result in solid solution, simple cubic structures or amorphous structures. The structure of the metastable system is, however, influenced by the equilibrium nature of the system. Those systems with many intermetallic compounds will form amorphous phases while those with no intermetallic alloys show a tendency to form solid solutions. At high temperature where atom mobility is significant, equilibrium phases will usually form. Metastable phases can be formed by neutron irradiation or by ion irradiation, ion implantation and ion beam mixing. Differences in the transformation process between ion irradiation techniques can provide insight into the mechanism governing metastable phase formation. For example, in ion irradiation experiments, the main result of the radiation is imparting damage to the lattice. However, in ion implantation, the implanted species provides a chemical alteration to the target as well. Ion beam mixing experiments are designed to follow the transformation by rapidly (far from equilibrium) altering the bulk content of the film. Metastable phases formed by irradiation usually occur by one of four types of transformations [26]: order → disorder crystal structure transformation: A → B crystal structure A → quasicrystal structure crystal structure A → amorphous structure The first three transformations will be briefly discussed and amorphization will be discussed in Sect. 9.7. For a more complete discussion of metastable phase formation, the reader is referred to [27].

9.6 Metastable Phases

461

9.6.1 Order–Disorder Transformations The order-disorder transformation and its role in phase stability was discussed in Sect. 9.3. However, radiation-induced disorder has been linked to metastable phase formation. In fact, many compounds are believed to undergo chemical disordering prior to amorphization under electron irradiation. Luzzi and Meshii [28] showed that of 32 compounds irradiated, all underwent chemical disordering and 15 amorphized. They concluded that irradiation-induced chemical disordering provided the driving force for amorphization, and cited the difficulty in forming the amorphous structure in pure metals as support for this argument. The linkage between disordering and amorphization also depends on the irradiation conditions, in particular the mass of the particle and whether damage is introduced via Frenkel pairs (electron irradiation) or in cascades (heavy ion irradiation). Comparison of the enthalpy for the order-disorder transformation to that for the crystalline-to-amorphous transformation shows that ΔHO-D ∼ 5ΔHc-a [16]. So in fact, the enthalpy change for disordering may be sufficient to induce amorphization. The role of disordering in the onset of amorphization will be discussed in Sect. 9.7. 9.6.2 Crystal Structure Transformations Numerous examples exist on the transformation from one crystal structure to another upon ion irradiation. One of the simplest examples is the transformation of pure nickel metal from fcc to hcp under irradiation. This transformation has been found to occur during irradiation with a variety of species including neutrons, chemically inert elements such as He and Ar, the metalloids P and As, as well as selfirradiation [29]. Observations on P-implanted high purity Ni [30] revealed an orientation relationship between the new hcp phase and the fcc matrix similar to that observed for martenistic fcc → hcp transformations. The transformation in Ni is thus believed to be martensitic. TEM examination of Sb-implanted Ni showed hcp particles extending 20 nm beyond the implanted depth, but dechanneling is present up to 130 nm, suggesting that the defect distribution is playing a role in the structure transformation. Ion irradiation has also been found to induce phase transformations between bcc and fcc phases in iron-based austenitic alloys [31]. The most prominent example is the fcc-to-bcc transformation of 304 stainless steel following implantation with 3 ×1016 Fe+ /cm2 at 160 keV. Although this dose amounted to an increase in the Fe alloy composition by only ∼ 1 at% (67 at% Fe nominal), the structure transformed from fcc → bcc. The orientation relationship was neither the Kurdjumov–Sachs nor the Nishijima–Wasserman relationships typically found in ion-irradiated steels [31], but instead obeyed the following relationship: (100)bcc ||(100)fcc

and [010]bcc ||[011]fcc .

(9.68)

Follstaedt [32] suggested that the transformation need not be occurring martensitically, but that the increased defect concentration and hence, diffusivity, may be responsible for the transformation. It should also be noted that this transformation is

462

9 Phase Stability Under Irradiation Fig. 9.19. Irradiationinduced solid solubilities for binary metal systems of positive heats of formation (from [33])

fundamentally different from that of nickel under irradiation in that the transformation is from the metastable state to the equilibrium structure, whereas in the case of Ni, the transformation is from the equilibrium fcc structure to a metastable hcp structure. The heat of formation of an alloy can have a strong influence on whether a metastable phase forms. Figure 9.19 shows the irradiation-induced solubilities for several binary metal systems as a function of the heat of formation, ΔHf . The samples were in the form of multilayers and were bombarded at 77 K by 400 keV Kr+ ions. All systems had positive values of ΔHf , meaning that in thermal equilibrium there is no, or only a limited miscibility of the components of the considered system. Note that the data points of the systems whose components have the same structures and of systems with components of different structure follow smooth curves. Both curves exhibit a rapid decrease from complete solubility to levels below 15 at% in a range of ΔHf of about 12 kJ/mol. However, even at large values of ΔHf , the solubility still has not disappeared. Metastable solid solutions can also form by displacement mixing at temperatures at which radiation-enhanced diffusion is sufficiently slow to maintain the supersaturated solid solution phase. Ion beam mixing of multilayered Ag–Cu targets form a continuous series of metastable solid solutions across the phase diagram. Although the phase diagram of the Cu–Ag system is a simple eutectic one with rather small solubilities of Ag in Cu and Cu in Ag, irradiation produced a single phase, metastable solid solution with the fcc structure across the entire Cu–Ag system [34]. Since ion beam mixing takes place mainly in the solid state, extended solid solutions can be achieved in nearly immiscible systems such as Ag–Ni. Even in the binary Au–Fe and Au–V systems which have more complex phase diagrams exhibiting a large solubility gap and several intermetallic compounds, respectively, and the bcc structure at the Fe– and V-rich terminal solid solutions, metastable solid solu-

9.7 Amorphization

463

tions form across both systems during ion beam mixing [35]. In all cases, the lattice parameters of the solid solutions vary smoothly with composition and show small or moderate deviations from Vegard’s law between the appropriate end-members. 9.6.3 Quasicrystal Formation The most novel metastable phases are the quasicrystalline phases, produced by ion irradiation of specific Al alloys. These phases show long-range order, but possess forbidden crystalline symmetries such a five or sixfold symmetry. The phase was discovered by Shectman et al. [36] at the National Bureau of Standards. Quasicrystals have positional order, but are neither periodically nor randomly spaced; instead, they are quasiperiodically spaced. This means that, given the position of one unit cell, the positions of the other unit cells are determined according to a predictable but subtle sequence that never quite repeats. Because these structures are highly ordered like crystals but are quasiperiodic instead of periodic, they have been called quasiperiodic crystals, or quasicrystals for short. The first quasicrystals formed by ion irradiation were in the Al–Mn system and examples extend into ternary and quaternary systems as well. In these initial experiments, the quasicrystal phase was formed by irradiating alternating layers of Al and Mn in the composition Al84 Mn16 with 400 keV Xe ions to doses of 2 – 10 ×1015 Xe/cm2 at 80 ◦C [37, 38]. Results showed that the icosahedral phase forms without a separate thermal treatment at or above 80 ◦C while the amorphous phase forms at 60 ◦C. The icosahedron is a regular polyhedron possessing twenty identical triangular faces, thirty edges and twelve vertices. The black pentagons on the surface of a soccer ball are centered on the vertices of an icosahedron. This observed dependence on sample temperature suggests that the icosahedral phase does not form within the dense ion cascade, but rather during subsequent defect evolution. Similar results have been achieved with freestanding Al–Fe multilayered samples [39], indicating that both multilayered and amorphous samples can be transformed to the quasicrystalline phase. In addition to temperature, the composition of the samples has an important effect on quasicrystal formation, establishing that quasicrystals are formed within a well-defined composition and temperature region.

9.7 Amorphization Irradiation can induce the formation of amorphous phases in alloys. Although the phase space available to an alloy is extremely large, only one point corresponds to an absolute minimum in free energy. This point represents the equilibrium phase. Given sufficient time, at any temperature greater than zero, the system will find that point and settle into the equilibrium phase. Nonetheless, there are generally other minima in the free energy phase space, which are of varying depths. These other minima correspond to metastable phases. Certain of these phases exhibit compositional short-range order (CSRO) very similar to that of the equilibrium phase but with different compositional long-range order. Similarly, the spatial arrangements

464

9 Phase Stability Under Irradiation

of the atoms on a small scale (topological short-range order, TSRO) can be very similar to the equilibrium phase but with different long-range order (such as fcc vs. hcp phases). In general, there may exist many phases with CSRO and TSRO that are nearly identical to the equilibrium phase. Common examples of such metastable phases include glasses and crystalline solids with a slightly different unit cell than the equilibrium. It has been suggested that in alloys with large negative heats of formation, disruption of chemical short-range order will lead to lattice destabilization and the formation of an amorphous phase [40]. In fact, the data on ion irradiation of intermetallic compounds supports just this sort of conclusion [22, 40]. Contradicting these observations are results of electron irradiation that show that complete longrange disordering often precedes the formation of an amorphous phase [26, 41]. For intermetallic compounds such as NiAl or FeTi, electron irradiation disorders but does not amorphize the compounds [42]. Irradiation with light ions produces much the same result as electron irradiation in that the amorphous phase is difficult to form, suggesting that disruption of CSRO is not adequate for lattice destabilization and that another mechanism must be responsible for amorphization such as topological disorder [42, 43, 44, 45, 46]. In fact, self-ion irradiation of Ni that induces a phase change from stable fcc to metastable hcp as discussed in Sect. 9.6, clearly has no chemical component and must be a result of the topological disorder introduced into the system by the Ni+ beam. The next two sections discuss the roles of heat of compound formation, crystal structure differences, solubility range of intermetallic compounds and the critical defect density on the formation of the amorphous phase. 9.7.1 Heat of Compound Formation and Crystal Structure Differences A good correlation exists between the heat of formation of a compound and the formation of amorphous phases in metal–metal systems [47], with large negative heats of formation tending to amorphize under irradiation. A plot of the ratio of the atomic radii vs. the heat of formation calculated using the Miedema model [48] shows where amorphization will occur (Fig. 9.20). In fact, alloys do not become amorphous if the heat of formation is greater than about +10 kJ/mol. However, the amorphous structure can be formed by ion mixing if the heat of formation is higher, e.g., Cr/Ag, Co/Cu, Fe/Cu and Co/Au. Specific compositions in the Au–Ir, Au–Ru and Au–Os systems, whose heats of formation range from +19 to +27 kJ/mol, were made amorphous by irradiation [33]. It has also been observed that crystalline phases of simple structures such as solid solutions or simple cubic structures form under irradiation, while amorphous phases are formed from more complex structures. This is explained by the short duration of the relaxation stage following the thermal spike. During the relaxation period, atoms attempt to re-arrange themselves. If the relaxation time is sufficient for precipitates to nucleate, crystalline phase formation may be achieved. The time required for nucleation is strongly influenced by the temperature, the crystalline structure of nuclei and the composition of the films that have been homogenized

9.7 Amorphization

465

Fig. 9.20. Ratio of atomic radii vs. the heat of formation of an equiatomic compound ( metal-metal crystalline, metal-metal amorphous, ◦ metal-metalloid crystalline, • metalmetalloid amorphous) (from [47])

with thermal treatments or ion beams. If the overall composition is not close to a simple crystal structure in the equilibrium phase diagram and there is not a strong chemical driving force (as well as mobility) to promote significant atomic motion, then crystalline phase formation may be inhibited. The role of structure difference in the propensity for irradiation-induced amorphization can be understood with the aid of a binary constitution diagram of an A–B alloy (Fig. 9.21a) a schematic free energy diagram for this alloy (Fig. 9.21b) and the corresponding polymorphic phase diagram (Fig. 9.21c) [49]. Note that the T0 curves in Fig. 9.21c are obtained from the crossing of the solid free energy curve with that of the liquid (or amorphous) curve at a given temperature. The T0α line defines the thermodynamic composition limits of the α -solution. When the concentration profile induced by mixing falls locally outside these limits, the α -solution is superheated with respect to the liquid (amorphous) phase and is not stable. Since melting is a local phenomenon not involving long-range diffusion, and since solids are not observed to withstand extensive superheating, it follows that observation of an α phase outside these composition limits represents an unstable state. Such a state will likely melt or amorphize before thermal spike evolution is complete. This leads to the first fundamental rule for solid phase formation. Johnson et al. [49] suggest that terminal solid solutions α and β can be formed up to the limits of the T0α and T0β curves (i.e., within the polymorphic phase diagram limits of α and β ). Solutions formed outside these limits are superheated and unstable against amorphization or melting. Secondly, intermetallic compounds with broad equilibrium homogeneity ranges (wide polymorphic limits in Fig. 9.21), and

466

9 Phase Stability Under Irradiation Fig. 9.21. (a) Binary constitution diagram of an A– B alloy. (b) Schematic free energy diagram for the alloy at temperature T2 . (c) Polymorphic phase diagram corresponding to the equilibrium phase diagram in part (a). The dashed lines show part of the original equilibrium diagram. Solid lines are representative T0 lines of each phase. The T0 lines define regions of polymorphic solid formation from the liquid state. Regions outside correspond to liquid or amorphous (polymorphic) states (from [49])

low-energy interfaces with α -solution or β -solution phases, may form in the prompt cascade provided that their respective growth kinetics allow high growth velocities. Compounds with narrow homogeneity range and complex chemically ordered unit cells should not form. Finally, amorphous phases are expected whenever the ion induced composition profile CB (z) lies outside the polymorphic limits of crystalline

9.7 Amorphization

467

Fig. 9.22. Possible configurations of an equilibrium, twophase alloy under irradiation at temperature T . Irradiation to an effective temperature, T1 gives amorphous and crystalline phases of different composition, while more intense irradiation to an effective temperature, T2 gives a single uniform amorphous phase (from [59])

phases. Amorphization may occur in addition when polymorphic limits permit compound formation but kinetics of compound formation or growth are slow. Martin [50] proposed a theory for amorphization that is similar in nature to that of Johnson. In this model, he adds the ballistic radiation recoil re-solution displacement jumps to thermally activated jumps to obtain an irradiation-altered diffusion equation. The practical effect of irradiation is then to cause the system to assume the configuration at temperature T that would be stable at a temperature T in the absence of irradiation: T = T (1 + DB /D ), where D is the thermally activated diffusion coefficient and DB is the diffusion coefficient including ballistic effects (Fig. 9.22). The theory predicts that irradiation of an equilibrium alloy of two solid phases at temperature T could raise the effective temperature to T1 , or under sufficiently intense irradiation to T2 . At T1 the irradiated alloy would at steady state be composed of amorphous and crystalline phases of different compositions. Irradiation intense enough to raise the effective temperature to T2 would produce a uniform amorphous alloy. 9.7.2 Solubility Range of Compounds and Critical Defect Density The tendency toward amorphization of the intermetallic compounds by irradiation correlates reasonably well with the degree of solubility within the phases. That is, alloys with limited solubility or a narrow compositional range show greater tendency for amorphous transformation. This correlation is also consistent with the concept that a critical energy or defect density must be created before the amorphous transformation can occur. If the total free energy of the defect crystalline state becomes greater than that of the amorphous state, a spontaneous transformation should occur. Associated with this critical free energy is a critical defect concentration. If this critical defect concentration can be reached under irradiation, then the crystal should

468

9 Phase Stability Under Irradiation

relax into the lower free energy (amorphous) state. This critical defect concentration has been estimated at 0.02 for silicon and germanium [51]. An estimate of the defect concentration required for amorphization can be made based on the increase in energy of lattice upon formation of a stable Frenkel pair. Each Frenkel pair will raise the energy of the alloy by an amount equal to the enthalpy of defect formation, ΔHi-v . The concentration of vacancy–interstitial pairs, Ci-v needed to increase the energy of the alloy by ΔHc-a can be estimated from the relationship: ΔHc-a = Ci-v ΔHi-v .

(9.69)

The magnitude of ΔHi-v for an fcc metal is approximately 5 eV, and ΔHc-a is approximately 0.06 eV/atom [16], giving the critical vacancy–interstitial concentration for amorphization as ∼ 0.01. However, such levels are not possible at reactor core component temperatures, but may be achievable in laboratory experiments conducted at temperatures where vacancies are immobile. The link between defect density and degree of solubility can be understood by referring to the free energy diagram in Fig. 9.23. Compounds with no or limited compositional range will undergo a greater increase in free energy than those with wide compositional range. The greater increase in free energy is due to the inability of the compound to exist in equilibrium outside the designated composition range. This is manifest in the narrow and steeply rising free energy vs. composition curves. For ordered phases (intermetallics) the increase is not only due to point defects, but anti-site defects in regions of localized non-stoichiometry. This proposed solubility rule is very consistent with Johnson’s thermodynamic analysis [49]. Note that for NiAl3 , only a slight deviation from stoichiometry is needed to result in a very large rise in the free energy. Therefore, the critical anti-site defect density would be low for NiAl3 as compared to NiAl. Anti-site defects may play a critical role in the amorphization process since calculations have shown that the critical defect density may be difficult to reach accounting for only point defects. However, since the defect concentration is strongly dependent on atom mobility and this is largely unknown in intermetallic compounds, accurate estimates of defect concentration are difficult to determine. Further, the critical defect density will be strongly temperature-dependent with higher concentrations required at higher temperatures. Further support for the existence of a critical defect density is provided by the observation that compounds that become amorphous during irradiation do not show evidence of prior dislocation loop formation [25, 52]. Although it has been assumed that the attainment of a critical defect concentration will cause an amorphous transformation, the high free energy associated with the point defects can also be relieved through the formation of a dislocation structure through the collapse of interstitial or vacancy clusters into small loops. However, observations show that either a material transforms directly to the amorphous state or forms dislocation loops. Since greater mobility is required for the formation of dislocation loops, and the maximum defect concentration associated with the nucleation of loops in irradiated metals is ∼ 10−4 [53], almost two orders of magnitude less than that for amorphization, indicates that defect mobility is a key factor in the amorphization process. This

9.7 Amorphization

469

Fig. 9.23. Ni–Al phase diagram (a) with hypothetical free energy diagram (b) at the irradiation temperature (from [19])

observation is consistent with the ease of amorphization in intermetallics where defect mobility is low, and the preferential formation of dislocation loops in pure metals and solid solution alloys where the mobility is high.

470

9 Phase Stability Under Irradiation

9.7.3 Thermodynamics and Kinetics of Amorphization In many respects, the C → A (crystalline-to-amorphous) transformation can be understood by relating it to melting by virtue of the similarity of these transformations. For example, amorphization is known to occur in a heterogeneous manner, similar to the first-order nucleation and growth process characteristic of melting. Also, Brillouin scattering studies have shown that intermetallics undergo a softening in the shear modulus, analogous to that observed at the onset of melting of many metals. As such, the C → A transformation can be considered to be a type of melting transformation. Okamoto et al. [54] wrote a comprehensive review of the physics of the crystalline-to-amorphous phase transformation. The role of irradiation in this transformation as presented in their paper is followed here. The liquid to glass transition is characterized by a temperature called the glass transition temperature, Tg . The glass transition is not a thermodynamic phase transition, but rather the point in the relaxation process where configurational equilibrium can no longer be achieved during the experiment. In this regard, it is more of a kinetic parameter that depends on the time-scale of observation. Free energy plots of the glass transition for perfect and defected crystals are shown in Fig. 9.24. The perfect crystal is shown by the bottom line and the defected crystals, denoted by the dashed lines, have higher free energies. The melting temperatures are given by Tm0 and Tmd , respectively. Also shown are two glass transition temperatures, Tg corresponding to an unrelaxed glassy state and Tk corresponding to the ideal glass

Fig. 9.24. Schematic plot of the Gibbs free energy as a function of temperature for a perfect crystal, the liquid phase and two defective crystalline states. Tm0 and Tmd are the thermodynamic melting temperatures of the perfect and defective crystals, respectively, Tg is the kinetic glass-transition temperature for the unrelaxed glassy phase and Tk is the ideal glass transition temperature (from [54])

9.7 Amorphization

471

transition temperature. Since the glass transition temperature is dependent on time, it is postulated that there exists some temperature, Tk below which the transition will never occur, and is known as the ideal glass temperature. Note that these points lie at a higher free energy than that of either the perfect crystal or the defected crystal. As described by Okamoto et al. [54], one of the simplest models of melting is due to Lindemann [55] who proposed that crystals melt when the root-mean-square + 2 ,1/2 of atoms from their equilibrium sites becomes (rms) thermal displacement, δvib large enough to encroach on nearest neighbors, or when the vibrational amplitude + 2 ,1/2 /rnn is about 50% of the interatomic spacing. Thus, melting occurs when δvib + 2 ,1/2 reaches a critical value equal to some fraction δcrit /rnn of the nearest neighbor spacing, rnn . In the harmonic Debye model of crystal lattices, the mean square thermal displacement for a perfect crystal at a temperature T above the Debye temperature, Θ0 is: + 2 , 36π 2 h¯ 2 T δvib = , MkΘ02

(9.70)

where h¯ is Planck’s constant, + k2 is, Boltzmann’s constant and M is the atomic mass. Since melting occurs when δvib reaches some critical value. Then from Eq. (9.70) the melting temperature of the perfect crystal is: Tm0 =

MkΘ02 + 2 , δcrit . 36π 2 h¯ 2

(9.71)

+ 2 , The + 2 total , mean-square atomic displacement is composed of thermal δvib and static δstat components, where the latter is due to defect structures such as point defects, anti-site defects, size mismatch between solute, solvent atoms in solid solution, defect clusters and impurities. The generalized form of the Lindemann melting criterion then becomes: + 2 , + 2 , + 2 , (9.72) δcrit = δstat + δvib , + 2 , where δcrit is a constant. Referring back to Fig. 9.24, this criterion , that + 2 the , + shows 0 2 crystal can be melted either by heating it to the melting + 2 , point, Tm ( δvib = δcrit ) or by increasing the amount of static disorder, δstat in the crystal until the free energy is equal to that of the liquid. As the damage level increases, the melting temperature of the defective crystal, Tmd defined by the intersection of the free energy curve with that of the supercooled liquid, decreases, as shown in Fig. 9.24. The maximum damage state will occur when the free energy curve of the defective crystal is tangent to that of the supercooled liquid, shown as the upper most dashed line in Fig. 9.24. + 2 , + 2 , = δcrit , or where Tmd = 0, is the theoretiThe state of maximum damage, δvib cal upper limit for damage accumulation in a defective crystal. , 9.25 shows + Figure 2 represents the a polymorphous melting curve for a defective crystal in which δstat

472

9 Phase Stability Under Irradiation

sum total of the effect of all defects in the crystal. The linear region follows from Eq. (9.72). Along the melting curve, where T = Tmd , Eq. (9.72) becomes: + 2 , + 2 , 36π 2h¯ 2 Tmd δcrit = δstat + , MkΘ02

(9.73)

which is written in the form of Eq. (9.71) as: Tmd =

MkΘ02 + 2 , δcrit , 36π 2 h¯ 2

where the Debye temperature of the defective crystal, Θ d is given as: + 2 , δ 2 2 , . Θd = Θ0 1 − + stat 2 δcrit

(9.74)

(9.75)

+ 2 , → 0, Θd2 → Θ02 , and Tmd → T0d . Note that Eq. (9.74) shows In a perfect crystal, δstat + 2 , that the proportionality between the melting temperature and δstat , Fig. 9.25, is related to the Debye temperature given in Eq. (9.75). Also, since Θd2 is proportional to the shear modulus, μd , the linear decrease in melting temperature also means that disorder-induced reduction + 2 , of the shear modulus is occurring with . From these proportionalities, we can the same functional dependence on δstat

Fig. 9.25. Generalized + 2disorder + 2 , T0 curve showing schematically the effects of static atomic , as measured by δstat , on the melting temperature of the defective crystal, Tmd . δmax and + 2 , + 2 , δcrit are the critical values of δstat for thermodynamic and mechanical melting (from [54])

9.7 Amorphization

write: Tmd μd Θd2 = = = 0 Tm μ0 Θ02

+ 2 , δ , . 1 − + stat 2 δcrit

473

(9.76)

If it were possible to relate the defects created by irradiation to the mean square displacement in the solid, then we could use Eq. (9.76) to determine the amorphization criterion directly. Since this is not possible, there are two alternative ways of determining the amorphization criteria. One is through disordering and another is through free energy change. Radiation-Induced Amorphization Driven by Disordering Recall that in Sect. 9.6 we determined that the disordering energy should be sufficient to drive the C → A transformation. In fact, the chemical rate theory of radiation-induced order-disorder transformation can be used to determine the cutoff temperature, below which amorphization can occur. In this model [56], the rate of change in the long-range order parameter consists of a disordering term due to irradiation and a thermal re-ordering term, similar to that in Sect. 9.3: dS −U = −ε K0 S + ν exp CA (1 − CA )(1 − S)2 dt kT −V S + CA (1 − CA )(1 − S)2 − exp (9.77) kT where U is the energy barrier for the A–B pair interchange, V is the ordering energy such that V = VAB − 1/2 (VAA +VBB) where VAB , VAA , and VBB are the bond energies for A–B, A–A and B–B pairs, respectively, and the remaining terms were defined in Sect. 9.3. The first term is the irradiation-induced disordering rate, and the second and third terms are the thermal re-ordering and disordering rates. An example of the variation of long-range order with temperature in the CuTi system is shown in Fig. 9.26 along with the variation of amorphization dose with temperature. Note that below about −53 ◦C, the order parameter drops to zero. This is the cut-off temperature, TC , which coincides with the onset of amorphization, Tc-a . Just above the cutoff temperature, dS/ dt is ∼ 0 and the relationship between the cutoff temperature and the damage rate, K0 , can be written by setting dS/ dt in Eq. (9.77) to zero: −U CA (1 − CA)(1 − S0)2 ε K0 S0 = ν exp kTC −V S0 − exp (9.78) S0 + CA (1 − CA )(1 − S0)2 , kT where S0 is the steady state value of the long-range order parameter. For typical values of V , the exponent inside the square brackets is of the order 10−5 to 10−21 and so the second term can be neglected, and the expression in Eq. (9.78) can be solved

474

9 Phase Stability Under Irradiation Fig. 9.26. Temperature dependence of (a) The long-range order parameter S/S0 , and (b) the critical amorphization dose for CuTi, irradiated with 1 MeV electrons (from [54])

for TC :

ν CA (1 − CA )(1 − S0)2 TC = U k ln ε K0 S0

−1 .

(9.79)

Equation (9.79) gives an estimation of the cutoff temperature, or the Tc-a temperature for a solid under irradiation. Note that it depends on the displacement rate and also on the number of replacements per displacement, ε . As such, the temperature at which amorphization will occur will depend on the irradiating particle and the dose rate. Figure 9.27 shows a schematic illustration of the temperature dependence of the critical dose for amorphization for various types of charged particles. Tc-a is the temperature below which complete amorphization can be achieved. Ta-c is the temperature beyond which the crystalline compound cannot be amorphized and is independent of irradiation conditions, and Tth is the thermal re-crystallization temperature. Okamoto et al. [54] describe the main kinetic features of irradiationinduced amorphization as follows: –

For a specified particle and dose rate, there is a temperature at which the two competing processes of damage production and recovery just balance. Below that temperature, damage production dominates recover and the crystal can be completely amorphized.

9.7 Amorphization

475

Fig. 9.27. Schematic illustration of the temperature dependence of the critical dose for amorphization for irradiation by various types of particles (from [54])

–

– – – –

Amorphization occurs homogeneously at low temperature, far from the critical dose rate and temperature. Heterogeneous amorphization occurs near the cutoff temperature. For fixed dose rate, Tc–a increases with increasing particle mass. Tc–a is a kinetic parameter that depends on the irradiation variables such as dose rate. Higher dose rates shift Tc-a to higher values. There is a temperature, Ta–c above which amorphization is impossible. Ta–c depends on the target temperature but not irradiation variables. Between Ta–c and Tth , irradiation can induce the A → C transformation and the dose required for the transformation is dose-dependent.

Figures 9.28a,b show two examples of the temperature dependence of irradiationinduced amorphization in NiAl and NiTi, respectively. Figure 9.29 shows how Tc–a varies with particle type at nearly equal dose rates. Clearly, irradiation with heavy ions can induce amorphization over a much larger temperature range than is possible by irradiation with electrons because the ions can transfer much more energy in a much smaller volume than can electrons. While electron irradiation in the ∼ MeV range produces isolated displacements (single Frenkel pairs), heavy ion irradiation results in cascades in which the effective displacement rate is high such that the damage rate outweighs the recovery rate. Relating the ordering process to the mean square static displacement, Okamoto et al. [54, 57] show that: + 2 , δstat α (1 − S2) , (9.80)

476

9 Phase Stability Under Irradiation

Fig. 9.28. Temperature dependence of the total displacement dose for ion-induced amorphization and crystallization of (a) crystalline and amorphous NiAl, and (b) crystalline and amorphous NiTi (from [54])

+ 2 , is proportional to the shear modulus, μ , then and since from Eq. (9.75), δstat μα (1 − S2 ). Figure 9.30 shows that amorphization of Zr3 Al occurs very near to the point where the straight line fit through data crosses the horizontal line for the amorphous alloy, showing that the onset of amorphization is related to a critical

9.7 Amorphization

477

Fig. 9.29. Temperature dependence of the critical amorphization dose for CuTi during irradiation with 1 MeV electrons and 1 MeV Ne, Kr and Xe ions, all at a dose rate of 10−3 dpa/s (from [54])

Fig. 9.30. Relative change in the shear modulus with increasing degree of disorder (1 − S2 ) in 1 MeV Kr+ irradiated Zr3 Al. The dashed line represents the relative shear modulus in the amorphous phase, and the vertical arrow indicates the onset of amorphization (from [54])

478

9 Phase Stability Under Irradiation

Fig. 9.31. Damage-dose dependence of the long-range order parameter, S in Zr3 Al during irradiation with 1 MeV electrons at 10 K and 320 K and with 1 MeV Kr at 295 K (from [54])

value of the mean-square chemical disorder (1 − S2) and from Eq. (9.80), the mean square static displacement. Another example of the role of disorder in amorphization is shown in Fig. 9.31 which gives the dose dependence of S for Zr3 Al during irradiation with 1 MeV electrons at two temperatures, and ions at 22 ◦C. The onset of amorphization is shown by the arrows, and although it occurs at different doses for the different particles and irradiation temperatures, the value of the order parameter is about the same. The significance of this observation is that while disordering kinetics differ between particles and temperatures, amorphization depends only on the magnitude of S and not how it is reached. Figure 9.32 [54, 57] shows an additional example of the correlation between the onset of amorphization and the rms static displacement for case of B implantation into Nb. When the mean square static displacement reaches a critical value, amorphization occurs. Radiation-Induced Amorphization Driven by Free Energy Amorphization can also be explained by considering the free energy of the transformation, as explained by Motta et al. [58, 59] and summarized here. The criteria for amorphization is that the free energy change upon irradiation, ΔGirr must be greater than that for the C → A transformation, ΔGac : ΔGirr ≥ ΔGac .

(9.81)

The term ΔGirr includes all of the defects created by irradiation and can be written as the sum of terms representing chemical disordering, ΔGdis and all other defects,

9.7 Amorphization

479

Fig. 9.32. Correlation between (a) average static displacement, δstat and (b) volume fraction of the amorphous phase vs. the concentration of B atoms implanted into Nb (after [32])

ΔGdef : ΔGirr = ΔGdef + ΔGdis = ∑ (C j E j − T ΔS j ) + ΔCAB NV − T ΔSdis ,

(9.82)

j

where C j is the concentration of defect j, E j is the formation energy, V is the ordering energy (defined earlier) and ΔS j and ΔSdis are the configuration entropy changes due to point defects and anti-site defects, respectively. The term ΔCAB is the change in the number of A–B pairs and is determined from the long-range order parameter,

480

9 Phase Stability Under Irradiation

Fig. 9.33. Plot of the dose to amorphization × square root of dose rate vs. 1/T . The lines are fit to the data and indicate that there are two regimes, an athermal regime at low temperature and a thermally activated regime at higher temperature (after [58])

S as: ΔCAB = N A 1 − S2 + B(1 − S) ,

(9.83)

where N is the number of lattice sites per mole and A and B are the fractions of atoms on the respective lattice sites in the ordered phase. The concentrations of defects is given by the defect balance equations given in Eq. (5.1). Equations (9.81), (9.82), and (9.83) and (5.1) can be used to determine a relationship between the dose to amorphization, the dose rate and the temperature. Motta determined this relationship for electron irradiation of Zr3 Fe to be: 1/2

Φa K0

i = B exp(−Em /2kT ) ,

(9.84)

i is the interstitial where Φa is the dose to amorphization, K0 is the dose rate, Em migration energy and B is a constant, and the results shown in Fig. 9.33 are found to be in good agreement with observations, shown in Fig. 9.34.

9.8 Phase Stability in Reactor Core Component Alloys The stability of phases in engineering alloys under irradiation is of great technological importance. Stainless steels are widely used in the cores of current

9.8 Phase Stability in Reactor Core Component Alloys

481

Fig. 9.34. Dose to amorphization for Zr3 Fe during electron and Ar+ irradiation (after [58])

and advanced reactor systems and have also been studied most comprehensively. Some 10 phases are observed to be affected by irradiation of austenitic stainless steels [60, 61, 62]. These phases can be grouped into three categories [60]: radiation-induced, radiation-modified, and radiation-enhanced. Table 9.2 gives the phases belonging to each category along with a crystallographic and morphological description of the phases. The radiation-induced phases include γ , G and Mx P phases and appear only under irradiation, but not under thermal conditions. The radiation-modified group consists of phases that occur during both irradiation and thermal aging and includes η (M6 C), Laves and M2 P (FeTiP). The radiationenhanced category consists of phases that regularly occur during thermal processing, but are either produced more rapidly or more abundantly at lower temperatures during reactor irradiation. Phases in this category include M6 C, M23 C6 and MC carbides and σ and χ intermetallic phases. Figure 9.35 provides a temperature-dose map in which the various phases listed in Table 9.2 are found to form. Note that while fluences of approximately 10 dpa are required for these phases to appear, the more important variable is temperature. In solution annealed and cold worked 316 SS, there is little evidence of significant radiation-induced precipitation below 370 ◦C. The only phase found to form in this regime is γ –Ni3 Si, and it has been observed in both light water reactor core components and following proton irradiation at 360 ◦C [63]. The γ phase has also been

-enhanced

-modified

-induced

Radiation

χ

Laves (A2 B) σ

M2 P (FeTiP) MC η (M6 C) τ (M23 C6 )

Laves (A2 B)

Cr3 P η (M6 C)

M2 P (FeTiP)

γ (Ni3 Si) G (M6 Ni16 Si7 )

Phase

Hexagonal, C14 P63 /mmc Same Cubic, B1 Fm3m Same Cubic, D84 Fm3m Same Tetragonal, D8b p4/mnm Cubic, A12 143m

Cubic, A1 Fm3m Cubic, A1 Fm3m Hexagonal, C22, P321 Tetragonal, S24 14 Cubic, E9, Fd3M

Crystal structure

– Rhombohedral Faulted lath

0.92 (c/a = 0.5) 1.08 0.47 (c/a = 0.77)

0.89

Same 0.88 (c/a = 0.52)

various

Same Various

Same Spherical Same Rhombohedral platelet

Thin lath

0.6 (c/a = 0.6)

Same 0.43 Same 1.06

Spherical Small rod

0.35 1.12

Lattice parameter (nm) Morphology

Table 9.2. Phases observed in austenitic stainless steel alloys after neutron irradiation (from [60] and [61])

various

Same Spherical Same Cube on cube or twin Same Various

0.05

Same ∼0

Same 0.7 Same 0.1

−0.05

∼0 0.1

−0.4

(1210)ppt ||(001)γ – Cube on cube or twin Various

−0.1 0.05

Volume misfit

Cube on cube Random

Orientation in γ matrix

482 9 Phase Stability Under Irradiation

9.8 Phase Stability in Reactor Core Component Alloys

483

Fig. 9.35. Dose and temperature dependence of precipitate phase formation in solution annealed 316 stainless steel irradiated in HFIR (after [61])

detected in 316 stainless steel irradiated in a fast reactor as low as 270 ◦C [60]. Between 400 and 550 ◦C, γ -Ni3 Si readily forms during fast reactor irradiations and is greatest in steels with higher Si and Ti contents. In mixed spectrum reactors in this temperature range, fine Cr-rich phases such as M23 C6 and M6 C form in 316 SS and Ti-rich MC forms in Ti-modified steels [60]. In the 500 to 600 ◦C temperature range, both radiation-induced and radiation-modified phases form, including the Gphase (M6 Ni16 Si7 ), M6 C Laves and phosphides and silicides. The G-phase volume fraction is a function of the Si, Ti and Nb content of the steel with volume fraction increasing with alloy composition. The appearance of these phases can be related to the effects of irradiation on phase stability. By far, the greatest effect of irradiation on precipitation in stainless steels is due to solute enrichment via radiation-induced segregation. Recall from Chap. 6 that irradiation of austenitic stainless steels causes the enrichment of Si and Ni at sinks and many of the phases appearing under irradiation are rich in one or both of these elements. Radiation-enhanced diffusion affects MC precipitation by enhancing its growth compared to that under thermal conditions. While it is expected that oversized phases are more stable under irradiation and undersized phases are less stable, of the phases given in Table 9.2, three have positive misfits of at least 10% and of those, only M6 C is stable under a wide range of irradiation conditions. Both MC and M23 C6 are oversized and will benefit from vacancy supersaturation, but also from the depletion of their main constituent, Cr, due to RIS. Conversely,

484

9 Phase Stability Under Irradiation

several of the phases that are undersized are induced or enhanced by irradiation: Laves, M2 P, γ . Clearly, the effect of solute segregation and other material and irradiation parameters play a large role in the phases that are stable under irradiation.

Nomenclature a A Ce Ci Cp D D˜ E j Em0 G ΔGp ΔG ΔGac ΔGirr ΔGdef ΔGdis h¯ ΔHf ΔHi-v ΔHc-a Jp k ko ks2 Kiv K0 L M n N px Q rc rp rj rnn R Rm

Lattice spacing Term relating to crystal structure dependence on ordering energy Matrix solute concentration Concentration of species i Concentration of solute in the precipitate Diffusion coefficient Interdiffusion coefficient Young’s modulus Migration energy for ordering of defect j Solute source term Free energy of formation of a precipitate Pseudo-free energy of formation of a precipitate Free energy change due to amorphization Free energy change due to irradiation Free energy change due to defects Free energy change due to chemical disordering Planck’s constant Heat of formation Enthalpy of defect formation Enthalpy for the crystalline to amorphous transition Precipitate nucleation rate Boltzmann’s constant Rate constant for the ordering reaction Sink strength Recombination rate constant Defect production rate Cell size Atomic mass Excess number of vacancies in a precipitate Atom number density Probability that a trap site is occupied by species x Activation energy for ordering Cascade radius Precipitate radius Recombination radius of specie j Nearest neighbor atom spacing Metal:metalloid size ratio Precipitate dissolution rate by ballistic mixing

Nomenclature

Rs R S Se Sj Sobserved S0 Sv Sx ΔSdis ΔS j t T TC Ta–c Tc–a Tg Tk Tm U V V0 VT Vc Vm Vi j x Xj Zα Zβ

α αj β βj δ + 2 ,1/2 δ + crit ,1/2 δ2 , + stat 2 1/2 δvib ε φ

Precipitate growth rate due to radiation-enhanced diffusion Gas constant Long-range order parameter Equilibrium value of order parameter Supersaturation of species j Observed long-range ordering parameter Steady state value of order parameter Vacancy supersaturation Solute supersaturation Configurational entropy change due to anti-site defects Configurational entropy change due to point defects Time Temperature Cut-off temperature Temperature above which crystal cannot be amorphized Temperature below which complete amorphization can be achieved Glass transition temperature Ideal glass transition temperature Melting temperature Energy barrier for ordering reaction Volume. Also, ordering parameter Activation energy when the long-range order parameter, S = 1. Energy reduction when a wrong A–B pair transforms to a correct A–B pair Cascade volume Molar volume Bond energy for species i and j Number of solute atoms in a precipitate Atom fraction of species j Number of α sites that are nearest neighbor to a β site Number of β sites that are nearest neighbor to a α site Constant in Eq. (9.22) Emission rate of species j Constant in Eq. (9.21) Capture rate of species j Fractional difference in volume of the precipitate relative to the matrix Critical value of means square displacement Amount of static disorder in the solid Root-mean-square thermal displacement Disordering efficiency Neutron flux

485

486

9 Phase Stability Under Irradiation

γ μ ν νj νc νw Θ Θ0 ρ ρp ρp0 ρ σ σD τ Ω ξ ζ

Particle-matrix interface energy. Also surface energy Shear modulus Poisson’s ratio Frequency factor for defect j Frequency factor for correct A–B pair Frequency factor for wrong A–B pair Re-solution rate of precipitate volume Debye temperature Density Precipitate number density Equilibrium precipitate number density Pseudo-equilibrium precipitate number density Parameter in Eq. (9.40) Displacement cross section Time constant Atomic volume Dissolution parameter in Eq. (9.32) Constant in Eq. (9.1)

Superscripts i v

Interstitial Vacancy

Subscripts d def dis e i irr m max p s th v x 0

Defective Defects Disordered Solubility Interstitials Irradiation Matrix Maximum Precipitate Solute Thermal Vacancies Solute atom Initial

Acronyms CSRO HFIR NHM

Compositional short-range order High Flux Isotope Reactor (Oak Ridge National Laboratory) Nelson–Hudson–Mazey

Problems

RED RIS TSRO

487

Radiation-enhanced diffusion Radiation-induced segregation Topological short-range order

Problems 9.1 A spherical precipitate grows via a random nucleation process at temperature T . The same precipitate grows under irradiation at the same temperature T . Under irradiation, the time to obtain the same volume fraction of precipitate is half that during pure thermal aging. Calculate the difference in the activation energy at this temperature between thermal and irradiated conditions for this transformation process. State key assumptions. 9.2 What phase is 304 stainless steel? Does radiation-induced segregation in 304 stainless steel tend to stabilize or destabilize this phase? Explain why. 9.3 For 316 SS under irradiation with a vacancy supersaturation, Sv = 104 and a solute supersaturation, Sx = 102 , find the interstitial to vacancy arrival rate ratio (βi /βv ) that will stabilize a precipitate phase that is oversized by 5% (δ = 0.05). Plot your results as a function of temperature from 573 to 873 K in increments of 100 K. Neglect the temperature dependence of Young’s modulus. 9.4 For a Ni–5%Al alloy undergoing shrinkage by recoil dissolution and growth by diffusion of the solute from solution: a) Determine the critical γ precipitate radius, below which growth occurs and above which shrinkage will occur. b) Compare your result to that expected when the precipitate size is governed by dissolution disordering. Use the following irradiation parameters:

φf = 1015 n/cm2 s (E ∼ 0.5 MeV) ρ = 1015 cm−3 ζ Ω = 10−4 nm ξ = 10 nm D = 10−15 cm2 /s 9.5 For the same alloy as in the last problem, plot the dependence of the maximum stable particle size on f , the fraction of atoms dissolved by a cascade for precipitates undergoing irradiation-induced re-solution. Make the plot for the range 0 < f < 1 and l = 10 nm. 9.6 Estimate the disordering rate due to irradiation for Ni–25Al (γ ) irradiated with 5 MeV Ni++ ions at a displacement rate of 10−3 dpa/s and with a disordering efficiency of 30. 9.7 A recent paper reports the discovery of a new microstructural defect aggreBH gate, termed a black hole because of its affinity for vacancies (zBH v > zi ).

488

9 Phase Stability Under Irradiation

Describe how the presence of these black holes along with the usual array of defect sinks will affect: a) Void nucleation rate b) Critical void size c) Void growth rate d) Incoherent precipitate (δ > 0) stability e) Incoherent precipitate nucleation rate. 9.8 In the nickel-rich end of the Ni–Al system, a solid solution of Al in Ni, known as the γ phase, has an fcc crystal structure. Near a composition of Ni–50Al, the β phase (bcc) is the stable structure. Given the information below, determine the window on Sv and βi /βv needed to form the NiAl (β ) phase from: a) A saturated solution of Al in Ni b) A supersaturated solution, Sx = 2.0 c) An undersaturated solution, Sx = 0.5. Irradiation temperature = 500 ◦C N = 0.35 E = 150 GPa aβ = 0.3574 nm aγ = 0.490 nm 9.9 Using the rules for amorphous phase formation, describe the relative ease of forming an amorphous phase in each single and two-phase region of the Ni–Al phase diagram. Explain your reasoning. 9.10 One of the theories of the formation of irradiation-induced amorphization requires that the vacancy and interstitial defect concentrations reach a level of 2%, at which point the affected volume will become amorphized. Determine whether this is possible in NiAl (β – bcc) by determining the migration enthalpy for interstitials at 300 K which would allow the point defect concentrations to reach this point. Assume a low sink concentration in the material and a displacement rate of 10−4 dpa/s. 9.11 Estimate the crystalline-to-amorphous temperature for NiAl3 for the following irradiation and material parameters under 5 MeV Ni++ ion irradiation: K0 = 10−3 dpa/s U = 0.1 eV S0 = 1.0

ν = 1013 s−1 ε = 30

References 1. Rehn LE (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier Science, New York, pp 17–33

References 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43.

489

Nelson RS , Hudson JA, Mazey DJ (1972) M Nucl Mater 44:318–330 Wilkes P (1979) J Nucl Mater 83:166–175 Brailsford AD (1980) J Nucl Mater 91:221–222 Wagner C (1961) Z Elektrochem 65:581–591 Lifshitz IM, Slyozov VV (1961) Phys Chem Solids 19:35–50 Frost HJ, Russell KC (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 75 Baron M, Chang H, Bleiberg ML (1977) In: Bleiberg ML, Bennett JW (eds) Radiation Effects in Breeder Reactor Structural Materials. TMS-AIME, New York, pp 395–404 Bilsby CF (1975) J Nucl Mater 55:125–133 Frost HJ, Russell KC (1982) Acta Metal 30:953–960 Frost HJ, Russell KC (1981) J Nucl Mater 103–104:1427–1432 Wollenberger H (1994) J Nucl Mater 2116:63–77 Abromeit C, Naundorf V, Wollenberger H (1988) J Nucl Mater 155–157:1174–1178 Russell KC (1984) Prog Mater Sci 28:229–434 Liou K-Y, Wilkes P (1979) J Nucl Mater 87:317–330 Nastasi M, Mayer JW, Hirvonen JK (1966) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge, p 342 Potter DI (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 213 Eridon J, Rehn L, Was G (1987) Nucl Instr Meth B 19/20:626 Brimhall JL, Kissinger HE, Charlot LA (1983) Rad Eff 77:273 Maydet SI, Russell KC (1977) J Nucl Mater 64:101–114 Russell KC (1979) J Nucl Mater 83:176–185 Mruzik MR, Russell KC (1978) J Nucl Mater 78:343–353 Cauvin R, Martin G (1981) Phys Rev B 32(7):3322–3332 Martin G, Bellon P, (1997) In: Ehrenreich H, Spaepen F (eds) Solid State Physics: Advances in Research and Applications, vol 50. Academic, New York, pp 189–332 Brimhall JL, Simonen EP (1986) Nucl Instr Meth B 16:187 Was GS, Eridon JM (1987) Nucl Instr Meth B 24/25:557 Was GS (1989) Prog Surf Sci 32(3/4):211 Luzzi DE, Meshii M (1986) Scr Metal 20:943 Johnson E, Wohlenberg T, Grant WA (1970) Phase Transitions 1:23 Grant WA (1981) Nucl Instr Meth 182/183:809 Johnson E, Littmark U, Johnson A, Christodoulides C (1982) Phil Mag A 45:803 Follstaedt DM (1985) Nucl Instr Meth B 78:11 Peiner E, Kopitzki K (1988) Nucl Instr Meth B 34:173 Tsaur BY, Lau SS, Mayer JW (1980) Appl Phys Lett 36:823 Tsaur BY, Lau SS, Hung LS, Mayer JW (1981) Nucl Instr Meth 182/813:1 Shectman D, Blech I, Gratias D, Cahn JW (1984) Phys Rev Lett 53:1951 Knapp JA, Follstaedt DM (1985) Phys Rev Lett 55(15):1591 Lilienfield DA, Nastasi M, Johnson HH, Ast AG, Mayer JW (1985) Phys Rev Lett 55(15):1587 Lilienfield DA, Mayer JW (1987) Mat Res Soc Symp 74. Materials Research Society, Pittsburgh, PA, p 339 Ossi PM (1977) Mater Sci Eng 90:55 Luzzi DE, Mori H, Fujita H, Meshii M (1984) Scr Metal 18:957 Pedraza DF (1987) Mater Sci Eng 90:69 Pedraza DF (1990) Rad Eff 112:11

490 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54.

55. 56. 57. 58. 59. 60. 61. 62. 63.

9 Phase Stability Under Irradiation Pedraza DF, Mansur LK (1986) Nucl Instr Meth B 16:203 Pedraza DF (1986) J Mater Res 1:425 Simonen EP (1986) Nucl Instr Meth B 16:198 Alonso JA, Somoza S (1983) Solid State Comm 48:765 Miedema AR (1973) J Less Comm Metals 32:117 Johnson WL, Cheng Y-T, Van Rossum M, Nicolet M-A (1985) Nucl Instr Meth B 7/8:657 Martin G (1984) Phys Rev B 30:1424 Swanson ML, Parsons JR, Hoelke CW (1971) Rad Eff 9:249 Brimhall JL, Kissinger HE, Pelton AR (1985) Rad Eff 90:241 Brimhall JL, Simonen EP, Kissinger HE (1973) J Nucl Mater 48:339 Okamoto PR, Lam NQ, Rehn LE (1999) In: Ehrenreich H, Spaepen F (eds) Solid State Physics: Advances in Research and Applications, vol 52. Academic, New York, pp 2–137 Lindemann FA (1910) Z Phys 11:609 Dienes GJ (1955) Acta Metal 3:549 Lam NQ, Okamoto PR, Li M (1997) J Nucl Mater 251:89–07 Motta AT, Howe LM, Okamoto PR (1999) J Nucl Mater 270:174–186 Motta AT (1997) J Nucl Mater 244:227–250 Mansur LK (1987) In: Freeman GR (ed) Kinetics of Nonhomogeneous Processes. Wiley, New York, pp 377–463 Maziasz PJ, McHargue CJ (1987) Int Mater Rev 32(4):190–218 Maziasz P (1993) J Nucl Mater 205:118–145 Was GS (2004) In: Proceedings of the 11th International Conference on Environmental Degradation of Materials in Nuclear Power Systems: Water Reactors, American Nuclear Society, La Grange Park, IL, pp 965–985

10 Unique Effects of Ion Irradiation

This chapter will focus on processes that are unique to ion bombardment of metals and alloys. Ion bombardment is important in fusion reactor systems in which the reaction products consist of energetic helium and hydrogen (deuterium or tritium) ions that impact the first wall and other components. In laboratory experiments, ion implantation, ion beam mixing and ion beam-assisted deposition are used to study ion–solid interactions and to create new phases and unique microstructures. The topic of ion beam modification of materials or ion–solid interactions in general is a broad subject, and a comprehensive treatment is beyond the scope of this text. (The reader is referred to several excellent texts and review articles on the subject, see for example, [1, 2, 3, 4, 5].) Rather, we will focus on processes that occur during ion–solid interactions and that result in unique microstructures or phases in the target, such as displacement mixing, preferential sputtering, Gibbsian adsorption, grain growth, etc., and the combination of these processes that together alter the target from its original state. Recall that ions not only create damage, but they contribute to a chemical change in the target by virtue of their presence. Processes affecting the surface structure and composition that are negligible under neutron irradiation (sputtering, recoil mixing, Gibbsian adsorption) can be very significant under ion irradiation. We will start with a brief introduction of ion irradiation techniques to set the stage for understanding the effects to be described later. The effects of ion irradiation on composition, microstructure and phase formation will then be presented. A final topic is the effects due to bombardment by gases at high doses and high temperature as will be experienced in the first wall of a fusion reactor, or at low temperature in a laboratory.

10.1 Ion Irradiation Techniques The modification of metal surfaces by ion beams can be accomplished by a variety of methods, each with its own advantages for particular situations. The principal methods include ion implantation, ion beam mixing, ion beam-assisted deposition and plasma ion implantation, and are shown schematically in Fig. 10.1a–d. Each of these techniques will be briefly described and considered for their capacity to alter the composition of the target.

492

10 Unique Effects of Ion Irradiation

Fig. 10.1. Ion beam surface modification by (a) direct ion implantation, (b) ion beam mixing, (c) ion beam-assisted deposition, and (d) plasma source ion implantation (from [3])

Ion implantation (II) is the bombardment of a target with a beam of ions in the energy range from a few hundred keV to several MeV. The beam is usually monoenergetic, contains a single charge state and is generally (but not always) mass analyzed. Due to the stochastic nature of the elastic collision process, the ions come to rest in a Gaussian distribution with the mean of the Gaussian centered about Rp , the projected range, with the FWHM ∼ 2.35ΔRp, where ΔRp is the standard deviation from the mean. Although it is a simple process, this technique has several disadvantages from the standpoint of modifying the surface composition. First, since the depth of the

10.1 Ion Irradiation Techniques

493

implanted distribution varies as E 1/2 , energies in the several hundred keV range that are achievable in the most common implanters, will result in projected ranges of less than 100 nm for most heavy ions. Energies in the MeV range are required to penetrate into the micrometer range. Second, sputtering will limit the concentration of the implanted specie to a value that is the reciprocal of the sputtering yield (see Sect. 10.2.1). Since sputtering yields of metals at these energies range from 2–5, the maximum concentration of implanted specie is 50 to 20%, respectively. The shape and location of the distribution can also be a drawback. In corrosion, where the composition of the top few monolayers is most important, the bulk of the modification occurs at considerably greater depths, leaving the surface lean in the implanted specie. When implantation induces a phase transformation, the effectiveness or efficiency of direct implantation is lesser still. Finally, it is often desirable to implant metal ions into pure metals or alloys to achieve a particular surface composition. As a practical matter, most commercial implanters can produce large currents of inert gases, but more elaborate measures are needed in order to produce metal ions at currents that are practical. Ion beam mixing provides an alternative to the shortcomings of direct ion implantation. Ion beam mixing (IBM) refers to the homogenization of bilayers or multilayers of elements deposited onto the surface of a target prior to bombardment. The idea behind IBM is to create a surface alloy by homogenizing alternate layers of the alloy constituents deposited in a thickness ratio so as to result in the desired final composition following mixing. IBM greatly relieves several of the shortcomings of ion implantation. First, the requirement of producing a metal ion beam is eliminated since noble gases can be used for mixing. Noble gases will not contribute a chemical effect in the solid and yet can be made into high current beams in most commercial implanters. Second, there is no restriction on the composition range since the final composition is controlled by the ratio of layer thicknesses. This also removes two other shortfalls of ion implantation, that of uniformity and surface deficiency of the implanted specie. Ion beam mixing results in a very uniform composition throughout the depth of penetration of the ion, including the very near-surface region that is problematical for ion implantation. Finally, if the elemental layers are made thin enough, the dose needed to achieve complete mixing can be orders of magnitude lower than that needed to produce concentrated alloys by direct implantation. If the process is carried out at low temperature, the result is often a metastable alloy in the form of either a supersaturated solid solution or an amorphous structure. The microstructure can then be controlled by subsequent annealing treatments. However, despite its many advantages, ion beam mixing still suffers from the same disadvantage of limited depth of penetration. The thickness of the surface is still governed by the projected range of the ion, which is in the 100 nm range for heavy ions of a few hundred keV. A solution to this problem lies in the technique of ion beam-assisted deposition. Ion beam-assisted/enhanced deposition (IBAD/IBED) refers to the growth of a film with the assistance of an ion beam. In this technique, a film is grown onto a substrate by physical vapor deposition concurrently with the bombardment by an

494

10 Unique Effects of Ion Irradiation

ion beam of low (∼1 keV) energy. The advantages of this method are numerous. First, there is virtually no limit to the thickness of film that can be modified since bombardment occurs during growth. Second, ion bombardment concurrent with vapor deposition provides for an atomically mixed interface, resulting in greater adherence. The composition gradient at the interface can be controlled by the deposition rate and the ion flux. Third, the enhanced mobility of the surface during growth allows for the control of grain size and morphology, texture, density, composition, and residual stress state. These properties are determined principally by controlling the atom deposition rate in conjunction with the ion flux (ion to atom arrival rate ratio), ion energy, fluence and species. Hence, pure metals, solid solution alloys, intermetallic compounds and a host of metal-based compounds can be grown by this technique. A final technique is plasma surface ion implantation (PSII). In this technique, the target is placed directly in the plasma source and is then pulse biased to a high negative potential (−40 to −100 keV). A plasma sheath forms around the target and ions are accelerated normal to the target surface across the plasma sheath. PSII has several potential advantages relative to conventional line-of-sight implantation including elimination of the need for target manipulation and beam rastering, elimination of target masking (retained dose problem), operation of the ion source hardware and controls are near ground potential, and easier scaling to large and/or heavy targets. All of these techniques involve energetic ion–solid interaction and the physical processes that constitute this interaction such as sputtering, Gibbsian adsorption, recoil implantation, displacement mixing, radiation-enhanced diffusion and radiationinduced segregation. These processes affect composition, microstructure and phase structure and form the basis for the observed changes in the physical and mechanical properties of the metal or alloy. Chapters 7, 8 and 9 described the microstructure and phase changes due to irradiation, and this chapter will focus on the composition effects and some additional effects unique to ion irradiation, such as grain growth, texture modification and surface morphology during high gas loading.

10.2 Composition Changes Under ion bombardment, a variety of processes occur, some of which are much more pronounced than in the case of neutron irradiation and some that are the same. Bombardment by heavy ions results in sputtering of atoms from the surface, inducing compositional changes in the near-surface region of the target. At temperatures between 0.3 and 0.5 Tm , Gibbsian adsorption causes changes in the composition of the first two atom layers, which can impact the sputtering process. The primary disordering mechanism is collisional or ballistic mixing which can be qualitatively classified into recoil implantation and cascade (isotropic) mixing. Recoil implantation refers to the direct displacement of a target atom by a bombarding ion. Indirect processes involving other target atoms are collectively called cascade mixing. Referring to experiments involving the implantation into a bilayer or a thin marker layer

10.2 Composition Changes

495

embedded in a monatomic solid, recoil implantation produces a shift and a broadening of a given initial profile while cascade mixing produces broadening. But in addition to collisional mixing, thermal processes may become important, leading to radiation-enhanced diffusion (Chap. 5). When the flux of defects to sinks becomes coupled to the flux of host atoms, radiation-induced segregation can occur, resulting in the accumulation or depletion of an alloy component at defect sinks (Chap. 6). The following subsections provide a development of the physical processes of sputtering, Gibbsian adsorption, recoil implantation and cascade mixing. Radiation-enhanced diffusion and radiation-induced segregation were described in earlier chapters and will be included only in combination with other processes to present a complete picture of composition changes under ion bombardment. 10.2.1 Sputtering Sputtering is a key element in determining surface composition under ion bombardment, primarily through the action of preferential sputtering. Different elements sputter with different probabilities, and the surface composition is a function of these probabilities. This section will briefly describe the process of physical sputtering, followed by a discussion of preferential sputtering as it affects surface compositional changes in alloys. Basic Model Surfaces of solids erode under ion bombardment. The erosion rate is characterized by the sputtering yield, Y , which is defined as the mean number of emitted atoms per incident particle. Y depends on the structure and composition of the target, parameters of the incident beam and the experimental geometry. For medium mass ions and keV energies, 0.5 ≤ Y < 20. In the sputtering process, atoms are ejected from the outer surface layers (Fig. 10.2). The bombarding ion transfers energy in collisions to the target atoms that recoil with enough energy to generate other recoils. Some of the backwarddirected recoils will intersect the surface with enough energy to escape the solid. It is these recoils that make up most of the sputtered yield, which is proportional to the number of displaced or recoil atoms. In the linear cascade regime, the number of recoils is proportional to the energy deposited per unit depth in nuclear energy loss [6, 7, 8, 9]. A collision cascade is linear if only a minor fraction of the target atoms within the cascade volume is set in motion. For a bulk cascade, this implies a low density of point defects generated. As applied to sputtering, it means that the sputter yield must be small compared to the number of target atoms located within the surface area affected by a bombarding particle. In practice, cascades in metals are close to linear except those generated by rather heavy ions bombarding heavy targets in the energy range from ∼10 keV to ∼1 MeV. The sputtering yield for particles incident on the surface can be expressed as: Y = Λ FD (E0 ) ,

(10.1)

496

10 Unique Effects of Ion Irradiation

Fig. 10.2. Schematic illustration of the re-direction of momentum from an incident ion to the backward direction resulting in sputtering

where Y is the number of atoms emitted per incident particle, E0 is the incident particle energy, Λ contains all the material properties such as surface binding energies and incident ion angular dependence, and FD is the density of deposited energy per unit depth at the surface and depends on the type, energy and direction of the incident ion and the target parameters Z2 , M2 and N. The derivation of Λ involves a description of the number of recoil atoms that can overcome the surface barrier and escape from the solid. Sigmund [6] has derived an expression for Λ using the Thomas–Fermi screening function:

Λ = 0.042/NU0 ,

(10.2)

where N is the atomic number density and U0 is the surface binding energy and can be estimated from the heat of sublimation. The deposited energy, FD is given as FD (E0 ) = α dE/ dx|n ,

(10.3)

where dE/ dx|n is the energy loss rate due to nuclear stopping and α is a correction factor that accounts for the angle of incidence of the beam to the surface and contributions due to large angle scattering events. The factor α increases with the angle of incidence due to increased energy deposition in the surface, and α also increases with M2 /M1 , again, due to greater energy deposition in the surface. Using the inverse square potential (see Eq. (1.159)), dE/ dx|n is evaluated to be: dE/ dx|n = NSn = N

π2 M1 Z1 Z2 ε 2 a , 2 M1 + M2

(10.4)

where N is the atom number density, Sn is the nuclear stopping power, a is the screening radius, ε is the unit charge, Z and M are atomic number and atomic mass, respectively, and the subscripts 1 and 2 refer to incident and target atoms, respectively. The nuclear stopping power calculated using a Thomas–Fermi cross

10.2 Composition Changes

497

section [10] is: Sn (E) = 4π aNZ1Z2 ε 2

M1 Sn (∈) , M1 + M2

(10.5)

where Sn (∈) is the reduced stopping power (from Eq. (1.142)), and the reduced energy, ∈ (from Eq. (1.137)) is: ∈=

a M2 E. M1 + M2 Z1 Z2 ε 2

(10.6)

For 1 keV Ar incident on Cu, a = 0.0103 nm and ∈= 0.008, and for 10 keV O incident on Cu, a = 0.0115 nm and ∈= 0.27. For ion energies between 1 and 10 keV, values of ∈ are in the range 0.01 to 0.3, or just below the plateau in dE/ dx|n . Using the energy-independent value of Sn (∈) of ∼0.39 eVcm2 (from Eq. (1.162)), gives dE/ dx|n ∼1240 eV/nm for Ar incident on C, and dE/ dx|n ∼320 eV/nm for O incident on Cu. Using the expression for Λ in Eq. (10.2), the sputtering yield in Eq. (10.1) becomes: Y = 0.528α Z1Z2

M1 Sn (∈) . U0 (M1 + M2 )

(10.7)

For Ar incident on Cu, NSn = dE/ dx|n = 1240 eV/nm, U0 ∼ 3 eV, α ∼ 0.25, Λ = 0.0165 nm/eV and N = 85 atoms/nm3, giving Y ∼ 5.1. Figure 10.3 shows the variation of the sputter yield with angle, atomic number of the ion, target atom– incident ion mass ratio and ion energy. Sputtering increases with departure from normal incidence because more of the ion energy is deposited close to the surface. The same is true for the dependence on Z of the ion for a fixed energy. Sputter yield is low at low energies because of the small amount of energy deposited in the surface. Similarly, since the elastic scattering cross section decreases with energy, the energy deposited in the surface region drops at high energies and the sputter yield falls. The result is a peak at intermediate energies where the energy deposition in the near-surface region is high. The sputtering yield can be used to determine the steady state concentration of the implanted specie [1] as follows. We assume that we are implanting an ion of element A in to a target of element B, where NA,B is the atomic concentration and SA,B is the sputtered flux of elements A and B. Then at any time, we have that: SB /SA = χ (NB /NA ) ,

(10.8)

where χ is the ratio of probabilities for sputtering a B atom off the surface to that for an A atom. The flux of incident A atoms, φA is related to the total sputtered flux by the sputtering yield:

φAY = SA + SB .

(10.9)

At steady state, the addition of A atoms by implantation equals that lost by sputtering so there is no net change in the total number of A atoms in the target and

498

10 Unique Effects of Ion Irradiation

Fig. 10.3. Dependence of sputter yield on (a) angle of incidence, β , where β is measured from the surface normal (from [8]), (b) atomic number of the incident ion (from [9]), (c) target atom–incident ion mass ratio through the factor α in Eq. (10.3) (from [8]), and (d) incident ion energy (from [7])

φA = SA . Substituting for SA into Eq. (10.9) yields SB = (Y − 1)φA . Substituting for SA and SB into Eq. (10.8) gives the steady state surface composition: NA /NB = χ (Y − 1)−1 .

(10.10)

For the case where χ = 1, Eq. (10.10) becomes: NA /(NA + NB ) = 1/Y ,

(10.11)

which indicates that the concentration of the implanted specie is determined directly by the sputter yield. Preferential Sputtering When energetic ions strike a target consisting of an alloy, not all of the elements of the target will be sputtered with the same yield. The yield of A atoms of an alloy per

10.2 Composition Changes

499

incident ion in the flux of sputtered atoms [11] is: YA =

∞ 0

σA (x)(CA (x)/Ω ) dx ,

(10.12)

where σ A (x) is the cross section for A atoms at a depth x ≥ 0 to be ejected from the surface, x = 0, into the region x < 0 per incoming ion, CA (x) is the atomic fraction of A in the alloy at depth x, and Ω is the mean atomic volume. We can also define the probability per unit depth, pA (x) that an A atom present at depth x is ejected by an incoming ion: pA (x) ≡ σA (x)/Ω .

(10.13)

The yield of A atoms then takes the form: YA =

∞ 0

CA (x)pA (x) dx .

(10.14)

The primary effects in alloy sputtering are those related to the individual sputtering events and the physical variables contributing to the sputter yield, and are all contained in the sputter probability, pA , which depends on the type and energy of the incoming ion, the type of the sputtered atom and its surface binding energy, etc. Since the values of the sputter probabilities, pi will differ for differing atomic species, preferential sputtering will occur. The secondary effects in alloy sputtering enter into Eq. (10.14) via the atomic concentration, CA , which gives the probability that a site is occupied by an A atom. As a consequence, the sputter yields of the alloying components will be affected through the factor CA (x) in Eq. (10.14). Practically, sputtered atoms come from a shallow layer (Fig. 10.1) with the contribution falling off exponentially with depth. The decay length is of the order of two atomic layers. Therefore, the integral in Eq. (10.14) can be replaced [6, 7, 12] by: YA = pACAs ,

(10.15)

where pA is the average total probability for an A atom present in the surface layer to be sputtered off per incident ion and CAs is the average atomic concentration of A in the surface layer, denoted by the superscript s. The thickness of this layer is not well-defined but should be taken as one or two atomic layers for determining CAs since the origin of sputtered ions is heavily weighted toward the first atomic layer. Differences in the sputter probabilities for component atoms in an alloy are caused by differences in the amounts of energy and momentum transferred to atoms of different masses, and surface binding energies. However, continued sputtering of a semi-infinite alloy target of uniform bulk composition must eventually lead to a steady state in which the composition of the flux of sputtered atoms leaving the surface equals the composition of the bulk alloy. Wiedersich et al. [11] have shown that bombardment of a binary alloy AB with a flux of ions φ (ions/cm2s) leads to an

500

10 Unique Effects of Ion Irradiation

atom removal rate given by: dN = φ (YA + YB ) . (10.16) dt Therefore, the rate at which the sputtered surface recedes can be calculated from the total rate of atom loss per unit area: δ˙ = dδ / dt = φ Ω dN/ dt = φ Ω (p Cs + p Cs ) , (10.17) A A

B B

where δ is the thickness of the surface layer removed by sputtering. They also showed that the net accumulation rate of species, i in a slab of solid at the surface of the sample, 0 ≤ x < x0 is: dNi (10.18) = φ Cib (α /Ω b ) − Yi , dt where Cib is the atomic concentration of component i of the bulk alloy, denoted by the superscript b, α is the volume removed per incident ion and Ω b is the average atomic volume of the bulk alloy. The net rate of accumulation of implanted ions is: dN0 = φ [1 − Y0] . (10.19) dt At steady state, the terms in the square brackets of Eqs. (10.18) and (10.19) must equal zero, giving: Y1 : Y2 : Y3 .... = C1b : C2b : C3b ...,

(10.20)

Y0 = 1 .

(10.21)

and

That is, the ratios of the alloy components in the sputtered flux are the same as those of the bulk alloy and their concentrations are just uniformly diluted by the re-emitted sputter ions. Note that the steady state flux of sputtered atoms contains no information on preferential sputtering. Information about preferential sputtering can be obtained from the steady state concentrations in the near-surface region via the approximation given in Eq. (10.15). Substituting Eq. (10.15) into Eq. (10.20) yields: p1 C1b C2s = , p2 C1s C2b

or

C1s C1b p2 = . C2s C2b p1

(10.22)

That is, after steady state is attained, the sputter probabilities are proportional to the ratio of the bulk and surface concentrations of the element in question. The sputter probability of the sputter ions can be obtained from the surface concentration: p0 ∼ =

1 . C0s

(10.23)

Lam and Wiedersich [13] have described the time evolution of preferential sputtering, PS on the near-surface composition for a binary alloy AB with psA > psB , i.e.,

10.2 Composition Changes

501

Fig. 10.4. Schematic description of the effect of preferential sputtering on the time evolution of the composition of the near-surface region of the sample and of the sputtered atom flux (from [13])

for the case where PS of A atoms occurs (see Fig. 10.4). Note that initially, the concentration of A atoms in the sputtered flux (top dashed line) is larger than in the bulk. However, as the surface composition changes (bottom dashed line) and the near-surface layer composition is altered, a steady state will be achieved after a certain bombardment time, when the composition of the sputtered atom flux becomes equal to the bulk composition, as dictated by the law of conservation of matter. That is, the surface concentration of A atoms will evolve to a steady state at which the higher sputtering probability of element A relative to element B, is offset by a lower A atom concentration. Consider a binary alloy, A:B such that CAb = CBb = 0.5. Then from Eq. (10.22) we have: CAs p = B . CBs pA

(10.24)

If the surface concentrations are measured to be CAs = 0.33 and CBs = 0.67, then we know that pA : pB = 2.0. Conversely, if we measure a steady state sputtered atom flux of A atoms to B atoms of 1.0 (YA : YB = 1.0), then all this tells us is that SA : SB = 1.0. That is, measuring the sputtered atom flux tells us nothing about the surface composition. We must make surface composition measurements directly and independently. 10.2.2 Gibbsian Adsorption Gibbsian adsorption (or thermal surface segregation) is the process by which the surface of an alloy re-adjusts itself to a composition different from that of the

502

10 Unique Effects of Ion Irradiation

bulk in order to lower the free energy of the alloy [14]. In metallic systems the change can be quite substantial, but the effect is confined to one or two atomic layers. The bulk composition is essentially unaffected because of the large bulkto-surface volume ratio. The re-adjustment occurs spontaneously at temperatures sufficiently high for diffusion to proceed at reasonable speed. Consider a surface layer of compositionCAs and CBs that differs from the bulk composition CAb and CBb . At equilibrium, the surface composition is related to the bulk composition [14] by: CAb CAs ΔHA = b exp − , (10.25) CBs kT CB where ΔHA is the heat of adsorption, defined as the enthalpy change associated with the exchange of an A atom in the bulk with a B atom at the surface. At elevated temperature, equilibrium is approached by a net flux, JA of A atoms described by: (10.26) JA Ω = (νAb→sCAb CBs ) − (νAs→bCAs CBb ) ξ , where ξ is the atomic layer thickness, νAb→s is the bulk-to-surface jump frequency and νAs→b is the surface-to-bulk jump frequency for atom A. The first term on the right is the flux of A atoms from the bulk to the surface and the second term is the flux of A atoms from the surface to the bulk. At equilibrium (JA = 0), or:

νAb→s CAs CBb = , νAs→b CAb CBs and substituting into Eq. (10.25) gives: ΔHA s→b b→s . νA = νA exp − kT

(10.27)

(10.28)

This says that the activation enthalpy for a surface segregating element (one that must have ΔHA < 0) for the jump back into the bulk is effectively increased by the heat of adsorption relative to the migration enthalpy in the bulk. The difference in concentration between the surface layer and the bulk is established and maintained by the reduced probability of thermally activated jumps of A atoms from the surface into the bulk. The enhanced surface concentration due to Gibbsian adsorption, GA will result in an increased loss of the segregated elements due to sputtering. Continued preferential loss of an element by GA requires that diffusion be high (T ≥ 0.5Tm ), but because sputtering enhances thermal diffusion, the effect of GA becomes significant at T ∼ = 0.3Tm . However, the athermal displacement mixing process will oppose GA. The effect of GA at steady state is to suppress the concentration in the alloy just below the surface layer to a value that maintains the surface layer concentration at the value dictated by preferential sputtering. Hence, under ion bombardment, the surface composition will be affected by both of these processes. Lam and Wiedersich [13] provided a schematic description of the dynamic behavior of the surface composition during ion bombardment resulting from the simultaneous effects of GA and PS. In the example shown in Fig. 10.5, Gibbsian adsorption

10.2 Composition Changes

503

Fig. 10.5. Schematic description of the simultaneous effects of GA and PS on the time evolution of the near-surface composition and of the sputtered atom flux (from [13])

results in a surface concentration of A atoms that is initially greater than the bulk level, shown by the step change in A atom concentration at the surface. This leads to enhanced preferential sputtering of A atoms since the sputtered atom flux is primarily from the first atom layer. Consequently, the concentration of A atoms in the subsurface layer will be reduced in an effort to re-establish thermodynamic equilibrium. After a time, t1 , the A atom concentration profile resembles the original in that there is a step-wise enrichment of A at the surface, but the surface concentration is reduced relative to the original and the concentration behind the step is reduced as well. With increasing bombardment time, the surface concentration of A continues to drop and the zone depleted in atom A increases in depth and width. Steady state is reached when the composition of the sputtered atom flux is equal to the bulk composition of the alloy. 10.2.3 Recoil Implantation The incoming ion beam imparts its momentum to the atoms (and electrons) of the solid. Hence, the momentum distribution of atoms during the displacement process is not isotropic and atoms will be re-located preferentially in the beam direction. This does not lead to any significant net atom transport in the beam direction because the solid will relax to approximately its normal density, i.e., the flux of recoiling atoms in the beam direction is compensated by a uniform flux of atoms due to relaxation in the opposite direction. In alloys, the relocation cross section and the range of the recoiling atoms depend on the charge and mass of the nucleus in such a way that generally the lighter component atoms will be transported relative to the

504

10 Unique Effects of Ion Irradiation

heavier components in the beam direction. This can be described as a flux of atoms of some of the alloy components toward deeper regions in the target, compensated by an opposite flux of the remainder of components to maintain atomic density at the proper value, i.e., the net flux of atoms is approximately zero across any plane parallel to the surface inside the target. The expression “recoil implantation” is used to describe the net transport parallel to the beam direction of some types of atoms relative to other types. The mechanics of recoil implantation have been developed by Sigmund et al. [15, 16, 17] and are summarized here. Consider the average implantation effect of a single ion (M0 , Z0 ) slowing down along a straight line to a well-defined range, R in a homogeneous binary alloy of components 1 and 2 , characterized by Mi ,Zi , and Ci with i = 1, 2, and C1 + C2 = 1. The number of i recoils created with energy (T , dT ) in element (x, dx) along its path is: NCi dxσ0i (E(x) , T ) ,

(10.29)

where E(x) is the ion energy at depth x and σ0i is the elastic scattering cross section between ions and i atoms. From LSS theory, the projected range of a recoil, Rp is:

T Rp = Ri (T ) γ0i E(x)

1/2 ,

(10.30)

where Ri is the path length and recoils are assumed to slow down on a straight line to a well-defined range, and γi j = 4Mi M j /(Mi + M j )2 . Then the total effect, Pi of the knock-on implantation is the integral of the number of recoils and their range: 1/2 R γ0i E(x) T dx σ0i (E(x), T )Ri (T ) dT . (10.31) Pi = NCi γ0i E(x) 0 0 Equation (10.31) is evaluated on the basis of power law scattering:

σi j (E, T ) = Ci j E −m T −1−m , i, j = 0, 1, 2, m 2(1−m) Mi Ci j = B1 ai j (Zi Z j )2m Mj

2/3 2/3 −1/2 ai j = B2 Zi Z j ,

0<m 0

C → 1 as t → 0

for x = 0

∞ −∞

C(x,t) dx = α , where α is the total amount of solute in the target. Assuming

that the layer is infinitely thin, the solution to Fick’s second law is: 2 −x α exp C(x,t) = √ , (10.46) 4Dt 4π Dt √ where the variance, σ 2 = 4Dt, the standard deviation, σ = 4Dt, and the full width at half maximum, FWHM = 2.35σ . From Eq. (10.44), the increment of FWHM due to cascade mixing is then:

√ 2 dE/ dx|n φ t 1/2 ∗ ∼ . ΔFWHM = 2.35 4D t = R Ed N

(10.47)

Note that the broadening of the thin film as described by ΔFWHM is proportional to (φ t)1/2 , or the effective ion mixing coefficient, 4Dt is proportional to φ t. Figure 10.8 shows that as predicted by Eq. (10.47), mixing given by 4Dt is proportional to the dose. Taking the example of 150 keV Kr+ bombardment of a Ni sample containing a thin film as in Fig. 10.7a, the dose needed to produce a ΔFWHM of 10 nm is: ΔFWHM = 10 nm ∼ =R

2 dE/ dx|n φ t Ed N

1/2 .

(10.48)

For dE/ dx|n = N σs T , then Eq. (10.48) becomes: 1/2

2σs T φ t . ΔFWHM = 10 nm ∼ =R Ed

(10.49)

For σs ∼ 1016 cm2 , T ∼ Ei = 150 keV, Ed ∼ 15 eV and R ∼ 1.5 nm, and the dose to cause a ΔFWHM of 10 nm is 8.5 ×1014 i/cm2 . If He+ is used instead of Kr+ , then the required dose is 3.5 ×1015 i/cm2 . Case 2: Pair of semi-infinite solids (bilayer) For a bilayer as shown in Fig. 10.7b, the boundary conditions are: C=0 C =C

for x < 0

at t = 0 ,

for x > 0

at t = 0 .

10.2 Composition Changes

509

Fig. 10.7. Schematic illustration of the effect of ion beam mixing on (a) a thin film, (b) a pair of semi-infinite solids (bilayer), and (c) a thin film of finite thickness (multilayer)

The solution to Fick’s second law subject to the boundary conditions is:

x C C(x,t) = . (10.50) 1 + erf √ 2 4Dt Figure 10.9 shows that as predicted by Eq. (10.50), mixing across a bilayer interface as described by 4Dt is, indeed, linear with dose for several bilayers systems, although the proportionality constant is system-dependent, as will be discussed later.

510

10 Unique Effects of Ion Irradiation

Fig. 10.8. Marker mixing data for several different markers in amorphous Si showing the relationship between the effective ion mixing diffusion coefficient, 4Dt, and the dose, φ t (from [1])

Case 3: Thin film of finite thickness (multilayer) For a layer of finite thickness, as shown in Fig. 10.7c, the boundary conditions are: C = C

for 0 < x < a

C=0

for x < 0 , x > a

and t = 0 , and t = 0 .

The solution is:

C x x−a C(x,t) = erf √ − erf √ . 2 4Dt 4Dt

(10.51)

Chemical Effects on Ion Beam Mixing Observations of mixing in binary systems reveals large differences in the amount of mixing that cannot be explained by ballistic effects. For example, mixing in the Cu– Au system is an order of magnitude higher than that in the Cu–W system [21, 22] and mixing of marker layers in Si and Ge varies significantly for elements of similar

10.2 Composition Changes

511

Fig. 10.9. Mixing of the interface vs. dose for several bilayer samples irradiated with 600 keV Xe++ ions at 77 K (from [20])

mass [23]. These systems are collisionally similar systems in that the ratio of the masses of the constituents is similar and so in a ballistic mixing model, they should behave similarly. Quite to the contrary, Fig. 10.9 showed that collisionally similar binary systems exhibited very different mixing rates. Further, mixing was occurring at 77 K where radiation-enhanced diffusion is suppressed. Johnson [24, 25, 26, 27, 28, 29] accounted for the chemical nature of the binary alloy components by first realizing that fundamentally, diffusion is driven by a chemical potential gradient, ∇μ (x) and only for ideal solutions does Fick’s law apply. More generally, for interdiffusion of two metals which form non-ideal solutions, one must relate ∇μ (x) to ∇C(x). This can be accomplished by replacing D by a modified D that accounts for the Kirkendall effect and describes diffusional

512

10 Unique Effects of Ion Irradiation

intermixing:

D =

D0ACB + D0BCA

2ΔHmix = D 1− kT

∂ ln γ (CA ) 1+ ∂ lnCA .

(10.52)

where D is the rate coefficient of unbiased mixing, γ is the activity coefficient and ΔHmix is the enthalpy of mixing given by: ΔHmix = 2δ CACB ,

δ = z[HAB − (HAA + HBB )/2] ,

(10.53)

where z is the coordination number (number of nearest neighbors) and Hi j is the potential between atom pairs, or pair enthalpies. Equation (10.52) simply says that random walk will be biased when the potential energy depends on the configuration. So mixing rates depend not only on the number of random walk steps per unit time, but also on the degree of Darken biasing. Figure 10.10 highlights the effect of ΔHmix on mixing rates for several bilayer systems. Equation Eq. (10.52) can be used to obtain a value of kTeff , the effective temperature at which diffusion occurs. [28] In the Pt–Au system, the value for kTeff is 1 – 2 eV. This means that the dominant contribution to ion mixing occurs when particle kinetic energies are of the order 1 eV! If mixing depends on the thermodynamic properties of the solid, then it should depend on the cohesive energy, ΔHcoh , which is a measure of how tightly bound

Fig. 10.10. Effect of the heat of mixing on the observed mixing rates for several binary metal systems following irradiation with 600 keV Xe++ ions at 77 K (from [24])

10.2 Composition Changes

513

Fig. 10.11. Effect of the average cohesive energy on ion mixing in several binary metal systems following irradiation with 600 keV Xe++ at 77 K (from [29])

atoms are in a solid. Indeed, if we plot d(4Dt)/ dφ vs. ΔHcoh , we note a strong correlation (Fig. 10.11). The energy range of interest, ∼1 eV correlates with the thermalized regime of a displacement cascade, which can be depicted as a thermal spike. The effect of thermal spikes on diffusion was treated by Rossi and Nastasi [30] starting with Vineyard’s thermal spike model [31] in which the non-linear Fourier equation for heat conduction in an isotropic and uniform medium is given as: ∇κ · ∇T = c

∂T , ∂t

(10.54)

where κ = κ0 T n−1 is the thermal diffusivity, c = c0 T n−1 is the specific heat capacity, κ0 and c0 are constants and n ≥ 1. At time t = 0, a cylindrical spike is introduced along an infinite straight line at constant energy density, ε , where the distance perpendicular to the axis of the cylinder is r. The initial condition for the temperature distribution is given by: Q=

c dT = (c0 /n)T n (r, 0) .

(10.55)

For zero initial ambient temperature, solution of Eq. (10.54) subject to boundary condition in Eq. (10.55), gives the temperature distribution in space and time:

T (r,t) =

nε 4πκ0t

1/n

exp(−c0 r2 /4πκ0t) .

(10.56)

514

10 Unique Effects of Ion Irradiation

Defining η as the total number of atom jumps in one spike per unit length of the spike, then analogous to thermal diffusion, we assume Arrhenius behavior for the jump rate, R such that R = A exp(−Q/kT ), then η is:

η=

2π r dr

A exp(−Q/T (r,t)) dt .

(10.57)

Integration of Eq. (10.56) yields:

η=

n3Γ (2n)Aε 2 , 8πκ0c0 Q2n

(10.58)

where Γ (2n) is the gamma function with argument 2n. For moderate temperatures, n = 1 and Eq. (10.58) becomes:

η=

Aε 2 . 8πκ cQ2

(10.59)

Referring back to Eq. (10.52) for a binary system with |ΔHmix | > 0, the effective jump rate at temperature T can be written as: Reff = A exp(−Q/kT ) [1 − 2ΔHmix/kT ] ,

(10.60)

and Eq. (10.57) becomes;

ηc =

2π r dr

A exp(−Q/kT (r,t)) [1 − 2ΔHmix/kT (r,t)] dt ,

(10.61)

where the subscript on η denotes chemical biasing. Taking n = 1 and carrying out the integral over the size and lifetime of the spike yields:

ηc =

Aε 2 (1 − 4ΔHmix/Q) . 8πκ cQ2

(10.62)

Since the activation energy scales with the cohesive energy, we take Q = −s2 ΔHcoh , where s2 is a constant. After a dose Φ (i/cm2 ), the total number of jumps in the solid is equal to ηc Φ /ρ , where ρ is the atomic density. The mixing rate is then given by: d(4Dt) = ηc rc2 /ρ , dΦ

(10.63)

where rc is a characteristic jump distance. Assuming that rc scales with the interatomic distance as rc = s1 ρ −1/3 , we obtain: d(4Dt) K1 ε 2 = 5/3 (1 + K2 ΔHmix /ΔHcoh ) , dΦ ρ (ΔHcoh )2

(10.64)

where K1 depends on κ , c and A, and K2 = 4/s2 . Equation (10.64) is plotted in Fig. 10.12 as the mixing vs. the ratio of ΔHmix /ΔHcoh for a large number of binary

10.2 Composition Changes

515

Fig. 10.12. Correlation between mixing and the ratio of ΔHmix /ΔHcoh for several metal bilayers irradiated with 600 keV Xe++ at 77 K (from [20])

systems and shows excellent correlation, indicating that the chemical effect of on beam mixing is indeed, strong even at temperatures where RED does not occur. With increasing temperature, RED contributes to mixing as well. Figure 10.13 shows the amount of intermixed silicon in a Si–Nb bilayer sample that was irradiated with Si+ ions [32]. At high temperature, the data follow an Arrhenius-type behavior with an activation energy of 0.9 eV. As the temperature is lowered, the amount of intermixing does not continue to drop, but levels out at a value that is determined by the ballistic mixing of the elements, which is temperature-dependent. Mixing induced by temperature only (thermal mixing) is shown by the solid curve on the left with an activation energy of 2.7 eV. The effect of radiation-enhanced diffusion is then the difference between the two plots that display Arrhenius behavior. Note that the low-temperature mixing is not due to

516

10 Unique Effects of Ion Irradiation

Fig. 10.13. Logarithm of the quantity of intermixed silicon vs. reciprocal temperature for a Nb–Si bilayer sample after a fluence of 1.2 × 1017 28 Si+ /cm2 . The solid line is fit to the data points of the sum of a temperature-independent part (nearly horizontal dotted line) and a thermally activated part (high slope dotted line) with an activation energy EA ∼ 0.9 eV (from [32])

an enhancement of diffusion by radiation, but rather to ballistic mixing. The total amount of mixing can be described by an effective diffusion coefficient [25] of the form: D = Dballistic + Drad exp(−Q/kT ) ,

(10.65)

where the first term on the right hand side is due to ballistic mixing and is temperature-independent, and the second term is due to radiation-enhanced diffusion and has an Arrhenius-type temperature dependence, where Q is an apparent activation energy. The temperature at which the two terms contribute equally to diffusion can be determined from Eq. (10.65) to be: Tc =

Q . k [ln(Drad /Dballistic )]

(10.66)

Assuming that there is a scaling relationship between the apparent activation energy and the cohesive energy of the matrix, ΔHcoh , i.e., Q = SΔHcoh , where S is a constant, then we obtain: Tc =

SΔHcoh . k [ln(Drad /Dballistic )]

(10.67)

10.2 Composition Changes

517

Fig. 10.14. Correlation between the average cohesive energy and the critical temperature, Tc at which mixing by radiation-enhanced diffusion equals that due to ballistic processes (from [33])

Figure 10.14 shows the critical temperature as a function of the average cohesive energy for several bilayer systems using a scaling factor, S = 0.1 [33]. Note that the critical temperature is linear with the cohesive energy, as predicted by Eq. (10.67). That the vacancy migration energy also scales with the cohesive energy means that radiation-enhanced diffusion is due to vacancy migration. In addition to homogenization of a target, displacement mixing is a very effective tool to study phase transformations under irradiation. Phase stability under irradiation was covered in Chap. 9, but ion beam mixing provides a unique opportunity to study ion-induced phase formation. Figure 10.15 shows how bilayer wedge

518

10 Unique Effects of Ion Irradiation

Fig. 10.15. Sample configuration, equilibrium phase diagram of Ni–Al and results of multilayered samples pre-annealed at 350 ◦C followed by irradiation with 500 keV Xe+ to a dose of 2 ×1015 cm2 (from [34])

samples can be made to cover the full range of composition in the Ni–Al binary system and how the phases develop as a function of composition. Figure 10.16 also shows that in most cases the phases formed are independent of whether the irradiation is by ion beam mixing, direct ion implantation of an inert element, or direct implantation of A into B or B into A. 10.2.5 Combination of Processes Affecting Surface Compositional Changes Accounting for the effects of all the processes described in the previous sections, Lam and Wiedersich [13] constructed a phenomenological model for bombardmentinduced composition modification by formulating a set of coupled partial differential equations describing the temporal and spatial evolution of defect and atom concentrations during ion bombardment of a binary alloy. The formulation was based on

10.2 Composition Changes

519

Fig. 10.16. Summary of microstructures in the Ni–Al system prepared by various ion beam treatments (from [35])

the set of diffusion and reaction rate equations, i.e., Fick’s second law with source and sink terms, describing the time rate of change of the alloy composition and defect concentrations,

∂ Cv = −∇ · (Ω Jv ) + K0 − R , ∂t ∂ Ci = −∇ · (Ω Ji ) + K0 − R , ∂t ∂ CA disp = −∇ · [(Ω JA ) − DA ∇CA ] , ∂t

(10.68) (10.69) (10.70)

where K0 and R are the locally and spatially dependent rates of production and disp recombination of vacancies and interstitials and DA is the diffusion coefficient caused solely by the displacement process. The time-dependent atom and defect concentration distributions can be determined by solving Eqs. (10.68) through (10.70) numerically for a semi-infinite target using appropriate starting and boundary conditions as described by Lam. [13, 36, 37, 38] This formulation covers the processes of DM, RED and RIS. Gibbsian adsorption and preferential sputtering can be accommodated in the model by treating the surface layer as a separate phase. Because of the structure of the phenomenological model, calculations can be made to determine the dependence of surface and subsurface compositional changes on material and irradiation variables as well as isolating the contributions of individual processes. However, because many of the parameters needed in the models are unknown, quantitative comparisons with experiment are difficult. Nevertheless, semi-quantitative modeling of bombardment-induced compositional redistribution in several binary alloys have been made. Wiedersich et al. [11, 34] provided a nice description of the effects of the different processes that occur during bombardment of an alloy and how those processes affect the surface composition. The calculations were performed with various combinations of preferential sputtering, displacement mixing, radiation-enhanced diffusion, Gibbsian adsorption and radiation-induced segregation included. Figure 10.17 shows the time evolution of the Cu concentration profiles and the location of the

520

10 Unique Effects of Ion Irradiation

Fig. 10.17. Time evolution of Cu concentration and the location of the surface in a Cu–40 at%Ni alloy bombarded with 5 keV Ar+ at 400 ◦C (from [11])

sample surface in Cu–40at%Ni bombarded with 5 keV Ar ions at 400 ◦C. Gibbsian adsorption causes an initial enrichment in the surface concentration of Cu (1 s). After 102 s, sputtering has preferentially removed Cu from the surface, resulting in a depletion of surface Cu relative to the bulk. After 4 ×103 s, steady state is achieved

10.2 Composition Changes

521

and the Cu concentration is depleted at the surface, but the depth profile continues to reflect the effect of GA. Note also the recession of the surface with increasing dose due to sputtering. Figure 10.18 shows the time dependence of the Cu concentration at the alloy surface. Note that in the absence of irradiation (curve 1), GA leads to a strong Cu enrichment in the first atom layer. Accounting only for PS and RED during irras to the steady state value, defined diation (2) causes a monotonic decrease in CCu by the sputtering probability ratio and the bulk composition. If GA is included (3), s increases rapidly at short times owing to radiation-enhanced adsorption, and CCu then decreases slowly to the steady state value. The inclusion of DM reduces the s decreases rapidly to effect of GA (4). Considering only PS, RED and RIS (5), CCu the steady state value due to the dominant effect of segregation. If GA is added (6) then the effect of RIS is masked. Finally, with the addition of DM (7), or when all s increases initially and then decreases toward the steady processes are included, CCu state value. The effect of different combinations of processes on the steady state Cu concentration profile is illustrated in Fig. 10.19.

Fig. 10.18. Effects of various combinations of Gibbsian adsorption (GA), preferential sputtering (PS), radiation-enhanced diffusion (RED), displacement mixing (DM), and radiationinduced segregation (RIS) on the time evolution of the surface concentration of Cu in Cu–40 at%Ni described in Fig. 10.17 (from [11])

522

10 Unique Effects of Ion Irradiation

Fig. 10.19. Effects of various combinations of the same five processes described in Fig. 10.18 on the steady state Cu concentration profiles (from [11])

10.2.6 Implant Re-Distribution During Ion Implantation The implantation example given in Fig. 10.17 to Fig. 10.19 was for bombardment of an alloy with an inert gas ion that plays no role as a chemical constituent of the alloy. In ion implantation, the concentration of the implanted ion is important to track, in addition to the effects of the various surfaces processes. A kinetic model was developed recently by Lam and Leaf [39] to describe the effects of these kinetic processes on the spatial re-distribution of implanted atoms during the implantation process. The effects of spatially non-uniform rates of damage and ion deposition, as well as the movement of the bombarded surface as a result of sputtering and introduction of foreign atoms into the system, were taken into account. The evolution of the implant concentration profile in time and space was calculated for various temperatures, ion energies, and ion–target combinations for a metal substrate B into which A atoms are implanted at a flux φ . The local concentrations of vacancies, B interstitial, A interstitials, A–vacancy complexes and free substitutional (A) solutes change with implantation time according to a system of kinetic equations [39] similar to those of Eqs. (10.68) through (10.70). Concurrently with the buildup of solute concentration in the host matrix, the surface is subjected to displacements both from sputtering and the introduction of foreign atoms into the system. Sputtering causes a recession of the surface while implantation causes an expansion. The net surface displacement rate is controlled by the competition between the rates of ion collection and sputtering.

10.2 Composition Changes

523

Fig. 10.20. Development of Al concentration profiles during 50 keV implantation at 500 ◦C. The normalized damage rate, K0 and ion deposition rate P are shown in the top plot and the surface displacements resulting from sputtering are indicated. Note that the concentration profiles are multiplied by factors shown in each plot (from [13])

The temporal and spatial evolution of the surface and subsurface alloy composition is obtained by solving this set of equations for a semi-infinite medium, starting from the thermodynamic equilibrium conditions. Sample calculations were performed for low and high-energy Al+ and Si+ implantations into Ni, since it is known from earlier studies that in irradiated Ni, Si segregates in the same direction as the defect fluxes whereas Al opposes the defect fluxes [40]. Re-distributions of Al and Si solutes in Ni during 50 keV implantation at 500 ◦C are shown in Fig. 10.20 and Fig. 10.21, respectively. s increases with time to a steady state value of In the Al-implantation case, CAl ∼50 at%, which is governed by the partial sputtering yield of the implant. This value

524

10 Unique Effects of Ion Irradiation

Fig. 10.21. Time evolution of the Si concentration profile during 50 keV implantation at 500 ◦C. The normalized damage rate, K0 and ion deposition rate, P are shown in the top plot. Surface displacements resulting from sputtering are indicated (from [13])

is substantially larger than that obtained in very high-energy implantation, where s sputtering is negligible and CAl is controlled by RIS. However, the total implant concentration remaining in the sample is significantly smaller because of sputtering.

10.3 Other Effects of Ion Implantation

525

Furthermore, the shape of the steady state implant profile is dictated by PS, which controls the boundary condition at the surface, and by RED and RIS. The evolution of the Si profile is rather different from that of Al, because of the different RIS behaviors. After a short implantation time, Si enrichment occurs at the surface because of RIS, and the Si distribution peak starts moving into the sample s increases monotonically, attaining interior (Fig. 10.21). With increasing time, CSi a steady state value of ∼100 at% at t ≥ 2 ×104 s. Unlike the Al case, the Si profile shows a significant shift of the implant distribution into the beyond-range region. This predicted translation of the Si distribution peak into the sample interior was consistent with experimental measurements by Mayer et al. [41] in Si-implanted Ni at elevated temperatures.

10.3 Other Effects of Ion Implantation 10.3.1 Grain Growth Ion-induced grain growth has been observed during irradiation of pure metals and multilayers. Liu and Mayer [42] observed the growth of grains of pure nickel films upon irradiation with inert gas ions, Ar, Kr and Xe in the energy range 150 to 580 keV. In their experiments, the grain size increased with dose until saturation at about 1 ×1016 i/cm2 . They found a nearly homogeneous grain size in the irradiated samples as compared to a wide spread in the grain size of thermally annealed samples. They also observed a dependence of the saturated grain size on ion species and only a weak dependence of grain size on ion dose at high doses (Fig. 10.22). The localized damage caused by the displacement spike in the vicinity of the grain boundary is the likely driving force for grain growth. The observed grain growth is explained by the re-ordering or growth of heavily damaged grains into neighboring, undamaged grains. The reduction in energy at a localized growing grain is equivalent to the difference between the energy released from the consumed region and the energy required to expand the grain boundary. The initially rapid grain growth can be explained by a larger probability of damaging an entire grain when the grains are small. As the irradiation process continues, the large grains consume the small ones and the average grain size increases. When the average diameter of the growing grains approaches the dimension of the damaged volume, the probability of highly damaging an entire grain by a single collision cascade is reduced, as is the chance of growing certain grains at the expense of others. Therefore, the grain growth rate gradually decreases with the increase of grain size. The grain growth rate during mixing of multilayered Ni–Al films is enhanced over that due to bombardment of co-deposited Ni–Al films of the same average composition by a factor of 2.2 (Fig. 10.23). This enhancement can be understood using the concept of the heat of mixing, using Johnson’s expression for the total number of atom jumps induced in a spike per unit length of a cylindrical thermal spike, η . Assuming that this value is proportional to grain boundary mobility, the

526

10 Unique Effects of Ion Irradiation

Fig. 10.22. Average grain diameter vs. dose for (a) 240 keV Ar, 310 keV Kr and 560 keV Xe ion irradiations of polycrystalline nickel films, and (b) 150 keV, 310 keV and 580 keV Kr ion irradiations of polycrystalline nickel films (from [42])

grain size, d can be related to the initial grain size, d0 and η in Eq. (10.64) as follows: 2 (d 3 − d03 )/φ αε 2 ΔHcoh [1 + K2 (ΔHmix /ΔHcoh )] .

(10.71)

10.3 Other Effects of Ion Implantation

527

Fig. 10.23. Ion-induced grain growth observed in 40 nm thick nickel, Ni–20at%Al multilayers and Ni–20at%Al co-evaporated films irradiated with 700 keV Xe++ ions (from [43])

Since ΔHmix = 0 for the irradiated co-evaporated films, the ratio of measured values of mobilities should be: (d 3 − d03 )ML / φ |ML = 1 + K2(ΔHmix /ΔHcoh ) . (10.72) (d 3 − d 3 ) / φ | 0

CO

CO

Given the cohesive energy and heat of mixing of a Ni–20at%Al alloy, the ratio in Eq. (10.72) is 3.0, as compared with the measured value of 2.2. These results indicate that the heat of mixing appears to play a role in ion-induced grain growth as well as ion beam mixing. 10.3.2 Texture There have been many reports of texture effects in ion beam mixed or ion beamassisted deposition of films. Alexander et al. [43] and Eridon et al. [44] found that mixing multilayers of Ni and Al in the composition Ni–20%Al resulted in the formation of the hcp and fcc (γ ) phases. The γ phase had a strong 111 texture and the hcp phase had a 001 texture. The textures were such that the close-packed planes of both phases were parallel to the film surface. These textures formed regardless of the angle of the ion irradiation with respect to the film. The formation of the texture seemed to be driven by the matching of the close packed planes. Ahmed and Potter [45] found that irradiation of Ni with Al to 1.2 ×1018 /cm2 resulted in 350 nm

528

10 Unique Effects of Ion Irradiation

grains of β phase oriented with respect to the underlying fcc nickel in accord with the Nishiyama relationship [46]. The development of texture during ion beam-assisted deposition can be correlated with the channeling directions of ions in the crystal lattice and the density of energy deposition would be inversely related to the depth of channeling. Thus, in an fcc crystal, the ease of channeling is in the order 110, 200, 111. Bradley et al. [47] have developed a model to explain the development of preferred orientation due to low-energy ion bombardment during film growth which is based on the difference in sputtering yields for different orientations rather than reorientation during recrystallization. Both effects are of course based on the same phenomenon of the variation of energy density with channeling direction. In this model, crystallites with high sputtering orientations are removed more rapidly and newly deposited material grows epitaxially in the low sputtering yield orientations. Thin films of PVD deposited materials normally grow with the planes of highest atomic density parallel to the substrate so fcc films have a 111 texture, bcc films have a 110 texture and hcp films have a 0002 texture (for ideal c/a ratios). The easiest channeling directions in each structure are as follows: fcc 110 , 100 , 111 bcc 111 , 100 , 110 hcp 1120 , 0002 Ion bombardment causes a shift in the preferred orientation to alignment of the easiest channeling direction along the ion beam axis. Thus, an ion beam at normal incidence on an fcc film will cause a shift in orientation from 111 to 110 texture. A beam incident at an angle will produce a different texture depending on the crystallography. The texturing effect appears to be most sensitive to high-energy beams because of the larger volume affected per ion and the deeper penetration. Experiments on ion bombardment during deposition of an Al film show that while Al forms a very strong 111 texture during physical vapor deposition, bombardment during deposition can induce an equally strong 110 texture that is driven by ion channeling [48]. 10.3.3 Dislocation Microstructure Ion implantation can induce the formation of a high dislocation density well beyond the implanted layer in response to high surface stresses caused by high doses of the implanted element [49]. Figure 10.24 shows the depth profile of the dislocation density in α -Fe resulting from implantation of various ions (C, Fe, W, Ar) at energies between 40 and 68 keV and to doses up to 1018 cm−2 . Note that while the projected ion range is less than 50 nm in all cases, the induced dislocation density peaks at between 5 and 10 μm and extends out to over 100 μm or more. The substructure is characterized by a dense dislocation network in which the dislocation density increases with dose and with the radius of the implanted ion. X-ray diffraction measurements show that the stresses exceed the yield stress and cause plastic strains in the range of 10%.

10.3 Other Effects of Ion Implantation

529

Fig. 10.24. Dislocation density vs. depth in α -Fe irradiated with 1) C: 40 keV, 1 ×1016 cm−2 , 2) C: 40 keV, 1 ×1018 cm−2 , 3) Fe: 68 keV, 1 ×1018 cm−2 , 4) W: 110 keV, 2 ×1017 cm−2 , 5) Ar: 50 keV, 2 ×1016 cm−2 , 6) Ar: 50 keV, 5 ×1016 cm−2 , 7) Ar: 50 keV, 1 ×1017 cm−2 . Irradiations 1–4 were pulsed and irradiations 5–7 were continuous (from [49])

The high density dislocation network created by ion implantation can induce recrystallization which can then affect the distribution of the implanted specie. Ahmed and Potter [45] performed a study of 180 keV Al implantation into pure Ni at 25 ◦C and at elevated temperatures (300 – 600 ◦C). At elevated temperatures, individual dislocation loops dominate the microstructure at the lowest fluences (∼1015 cm−2 ). These loops bound collections of interstitial atoms or vacancies, defects caused by the energetic Al ions penetrating the nickel structure and displacing atoms from their lattice sites. The loops climb with further implantation, intersect and react with other loops, and form complex dislocation networks after a dose of 2.1 ×1017 Al/cm2 . By a dose of 3 ×1017 Al/cm2 , three-dimensional aggregates of vacancies are present. The composition profile of Al implanted into Ni is relatively independent of temperature between 23 and 600 ◦C and for doses less than 1018 cm−2 . However, at higher doses, gross changes in the implanted distribution occur with the profile flattening and a considerable amount of Al transported to greater depths (Fig. 10.25). The same occurs following aging of room temperature implantations at 600 ◦C for 15 min. The microstructures developed at depths greater than the range of the 180 keVAl+ ions, ∼100 nm, play an important role in determining the stability of the implanted concentration profiles. Dislocation loops are present at depths near 300 nm following room temperature implantation. These loops are faulted Frank loops, 5 – 10 nm in diameter and their number density increases with fluence, reaching ∼4 ×1016 cm−2 at 3 ×1018 cm−2 .

530

10 Unique Effects of Ion Irradiation Fig. 10.25. Peak aluminum concentration plotted vs. fluence for implantation of aluminum into nickel at 500 ◦C (from [45])

However, the dislocations behind the implanted layer are removed when the material is heated to 600 ◦C. This occurs by re-crystallization, which is also responsible for the re-distribution of implanted Al. The following describes the processes occurring. Following room temperature implantation, an amorphous phase extends to a depth of ∼160 nm. Small crystal of β and γ extend from 160 nm to ∼300 nm and from ∼300 nm to ∼400 nm, respectively. Dislocations and dislocation loops extend beyond this to depths of >800 nm. Aging at 600 ◦C following room temperature implantation or implanting at high temperatures causes re-crystallization of the fine grain structure to depths of ∼ 800 nm to ∼1000 nm. In both instances, aluminum atoms must move through relatively pure nickel to accomplish the re-distribution, which is only possible if some fast diffusion process occurs. This is afforded by the small grains which form upon re-crystallization of the heavily dislocated region beyond the implanted layer and provide high angle grain boundaries for abnormally fast diffusion. The composition reaches a plateau by virtue of the limited extent of the re-crystallization. Figure 10.26 shows that the re-distribution only occurs above a threshold dose indicating the role of the radiation damage in the re-crystallization process. This example serves to tie together the roles of the implanted specie, the character of the radiation damage and the processes (re-crystallization and abnormally fast diffusion) that can be affected by implantation fields.

10.4 High Dose Gas Loading: Blistering and Exfoilation The first wall and divertor of a fusion reactor are expected to be subject to high fluxes of moderate to low-energy deuterium and helium ions created as fusion reaction products. Below 1 MeV, helium comes to rest approximately 1μm below the surface and extended exposure at high flux can lead to very high levels of

10.4 High Dose Gas Loading: Blistering and Exfoilation

531

Fig. 10.26. Aluminum concentration vs. time at 600 ◦C for fluences between 0.6 and 3.0 ×1018 i/cm2 . The phases observed in the implanted layers, symbols on curves, and those expected based on the equilibrium phase diagram (right side ordinate) are shown (from [45])

helium. At the expected temperatures (400 – 700 ◦C) and aided by the high defect concentration due to radiation damage, He will be mobile and will form bubbles as discussed in Chap. 8. The growth and coalescence of bubbles leads to the formation of blisters resulting in exfoliation of the surface as shown in Fig. 10.27. Figure 10.28a illustrates the result of high He loading a short distance beneath the surface of a metal. The bubbles are constrained to a narrow band of solid beneath the surface. There, they may grow and either coalesce to form larger bubbles or cause interbubble fracture due to the stresses between the bubbles (Fig. 10.28a). A cross sectional image of the subsurface region of a nickel sample bombarded with a high dose of He, Fig. 10.28b shows that the bubble microstructure is confined to the near-surface region. Stresses arise because the bubbles are not in equilibrium. That is, pressure due to the gas in the bubble is not balanced by the stress due to the surface tension, resulting in a radially directed stress, σrr on the bubble:

σrr = p − (2γ /r) .

(10.73)

Wolfer [52] developed an expression for the average stress field between bubbles: 2γ 4πρB 1/3 2/3 σ p = fHe − S F(S) , (10.74) μ μρΩ μΩ 3

532

10 Unique Effects of Ion Irradiation

Fig. 10.27. Surface topography of polycrystalline nickel irradiated with different doses of 100 keV He+ ions: (a) 2 × 1018 4 He/cm2 at normal incidence, (b) 2 × 1018 3 He/cm2 at normal incidence, (c) 1 × 1019 3 He/cm2 at normal incidence, (d) 2 × 1019 3 He/cm2 at 60◦ from normal, (e) 1.2 ×1020 4 He/cm2 at normal, and (f) 3.4 × 1019 3 He/cm2 at 60◦ from normal (from [50])

where μ is the shear modulus, fHe = mρB Ω , m is the number of gas atoms in a bubble, ρB is the bubble density, Ω is the atomic volume of the metal atoms, ρ is the helium density in the bubbles, γ is the surface energy and S = fHe /ρ The function

10.4 High Dose Gas Loading: Blistering and Exfoilation

533

Fig. 10.28. (a) Coalescence of bubbles below the surface of a sample loaded with a high dose of helium. (b) Cross section of a high dose, He-implanted surface layer of nickel showing the dislocations (deep), bubble lattice (middle) and connected channels (near-surface) (from [51])

F(S) is defined for a random array of bubbles and for ρ ∼ 1.0 as: F(S) = (0.827S1/3 − S)−1 .

(10.75)

534

10 Unique Effects of Ion Irradiation

Since the ultimate tensile strength determines both the ductile, transgranular fracture of fcc metals and the transgranular cleavage fracture of bcc and hcp metals, and is about 0.003 μ for fcc metals and roughly 0.01 μ for bcc metals, then σ ∼ 0.01μ . The corresponding helium concentrations needed to reach the stress to cause fracture between bubbles due to the stress are shown in Fig. 10.29, and for ρ = 1, the critical helium concentration is ∼20 − 40%. Wolfer also identifies another stress, the lateral stress, σL that is in the plane of the bubbles parallel to the surface (Fig. 10.30). The lateral stress depends on the swelling rate, S˙ according to:

σL =

˙ −SE , (1 − ν )

(10.76)

where E is the elastic modulus and ν is Poisson’s ratio. Blister formation is then a two-step process. Fracture starts at the depth, tB below the surface where σ is a maximum by growth of the bubbles to a point where the local stresses are sufficient to crack open the plane adjoining the bubbles. The penny-shaped crack then spreads until a diameter, DB is reached where the buckling condition is satisfied by the existing lateral load:

Fig. 10.29. Critical implanted He concentration vs. He concentration in the bubbles for the case of random bubbles (from [52])

10.5 Solid Phases and Inert Gas Bubble Lattices

535

Fig. 10.30. Schematic cross section of the He-implanted layer with gas bubbles and definitions of the lateral stress and the interbubble stress (from [52])

DB = 1.55 where P = −

μ , (1 − ν )P

(10.77)

σL dtB

(10.78)

tB 0

Note that experiment has identified the relationship between the blister base diameter and its thickness to be DB ∼ tBm , and this relation supports the lateral stress as the cause of blister formation [52]. Alternatively, the penny-shaped crack can continue to extend until detachment occurs, resulting in flaking and exfoliation as shown in Fig. 10.27. Very high doses of helium or implantation at high temperature often result in a sponge-type structure in which the surface consists of a series of pits as shown in Fig. 10.31. At very high temperature where bubbles are mobile, the pits may be the result of bubble intersection with the surface. However, high dose ion implantation can led to severe topological surface changes and this is the subject of much investigation.

10.5 Solid Phases and Inert Gas Bubble Lattices Implantation of noble gases to high doses at room temperature can lead to a different phenomenon: solid bubbles. Ar, Kr and Xe implanted into a variety of host metals have been observed to form solid bubbles consisting of crystals of the implanted

536

10 Unique Effects of Ion Irradiation Fig. 10.31. Holes in the surface of Nb irradiated with (a) 1.2 × 1020 He/cm2 at 23 ◦C and (b) 3 × 1017 He/cm2 at 823 ◦C (from [53])

noble gas. In Ni and Al, gases precipitate as solids with the same crystal structure as the host lattice and epitaxially aligned with the matrix. The solid phase forms at doses in the range of 1020 m−2 and the precipitate size is about 1.5 nm in Ni and up to 4.7 nm in Al [54, 55]. The lattice parameter of the precipitates is larger than that of the host and increases with the atomic mass of the inert gas. The lattice parameter increases with dose and tends toward a saturation value as shown in Fig. 10.32. Precipitate densities can be very high, in the range of 1024 m−3 . The average pressure of the solid gas can be determined from the average gas density, the lattice constant and the equation of state for the gas and is estimated to reach values in excess of 40 kbar. While the pressure required to solidify the gas at room temperature depends on the gas (8 kbar for Kr and 11.5 kbar for Ar), the calculated values are in excess of these amounts by several times. The inert gas is held in the solid state by the interatomic forces between the Kr–Kr and the Kr–Ni atoms, for the case of Kr in Ni. As the precipitate size increases, the average spacing between the gas atoms increases, decreasing the magnitude of the Kr–Kr interaction. Eventually, the decrease in gas pressure allows melting of the solid Kr. Implantation of high doses of Kr into amorphous TiCr resulted in the precipitation of crystalline Kr as in the case of crystalline

Nomenclature

537

Fig. 10.32. Lattice parameter of solid noble gas precipitates of Xe, Kr and Ar in nickel and of Kr in aluminum, as a function of fluence and implanted at room temperature (from [54] and [55])

metal hosts, but in this case, the solid Kr precipitates induced local crystallization of the host as a bcc structure. High dose implantation at room temperature can also lead to bubble lattice formation similar to the void lattices described in Chap. 8. Bubble lattices have been observed in Cu, Ni, Au, Ti and stainless steel irradiated with He or Kr. In fcc lattices, the bubbles form in densely packed rows parallel to the matrix {111} trace directions [56], and can be described by a lattice constant of order 7.6 nm, corresponding to a bubble density of ∼1025 m−3 . In hcp lattices, the bubble alignment is parallel to the basal plane, similar to that found for void ordering [57]. The formation of a bubble lattice is independent of the inert gas used and whether the gas atoms are present in bubbles in a gaseous or solid form.

Nomenclature a c dE/ dx|n d D DB D∗ D

Screening radius. Also nearest neighbor distance Specific heat capacity Ci Concentration of atom of type i Energy loss rate due to nuclear stopping Grain size Diffusion coefficient Blister diameter Effective diffusion coefficient Modified diffusion coefficient accounting for diffusional intermixing

538

E Ecoh Ed Emix F FD Hi j ΔHcoh ΔHA ΔHmix Ji k K0 m M N p pi pi P Pi Q Qi rc R

Rd Rp Rrecoil ΔRp S Si Sn SX t tB T Teff U0 Y z Z

10 Unique Effects of Ion Irradiation

Energy. Also Young’s modulus Cohesive energy Displacement energy Energy of mixing Displacement rate in dpa/s Deposited energy Potential energy between atom pairs of type i and j Cohesive energy Heat of adsorption Heat of mixing Flux of atoms of type i Boltzmann’s constant Defect production rate Number of gas atoms in a bubble Atomic mass Atom number density Gas pressure in a bubble Sputter probability of atom of type i Average total sputter probability of atom of type i Load Total effect of recoil implantation, Eq. (10.31) Activation energy Equivalent number of i atoms recoil implanted over a depth Rp Characteristic jump distance in a thermal spike Ion range. Also root mean square of an atom in a collision cascade Also vacancy–interstitial recombination rate. Also jump rate in thermal spikes Displacement rate in #/cm3 s Projected range Recoil range Standard deviation of the projected range Scaling factor Sputtered flux of atom of type i Nuclear stopping power Sputtered flux of element X Time Blister shell thickness Temperature. Also energy transferred in a collision event Effective temperature at which diffusion occurs Surface binding energy Sputter yield Coordination number Atomic number

Nomenclature

α χ δ ε ∈ φι γ Γ η κ λ Λ μ ν νis→b νib→s ρ ρB σd σs σ0,i σi σL σ Ω ξ

Constant in Eq. (10.3) Ratio of probability of sputtering a B atom to that for an A atom Thickness of surface layer removed by sputtering Unit charge. Also the energy density in the cascade Reduced energy Flux of atoms of type i Activity coefficient. Also surface energy Total jump frequency Number of atom jumps in a thermal spike per unit length of the spike Thermal diffusivity Jump length Factor in sputtering yield Eq. (10.2) containing material parameters Shear modulus. Also chemical potential Number of displacement per primary knock-on atom. Also Poisson’s ratio Surface-to-bulk jump frequency for atom i Bulk-to-surface jump frequency for atom i Atom density Gas bubble density Displacement cross section Scattering cross section Elastic scattering cross section between ions and i atoms Surface ejection cross section for atoms of type i Lateral stress in the solid Average stress Atomic volume Atomic layer thickness

Superscripts b s

Bulk Surface

Subscripts A B d P s

539

Adsorption Bubble or blister Displacement Projected Scattering

540

10 Unique Effects of Ion Irradiation

Acronyms CO DM GA FWHM IBAD IBED IBM II ML PS PSII RED RIS

Co-evaporated Displacement mixing Gibbsian adsorption Full width at half maximum Ion beam-assisted deposition Ion beam-enhanced deposition Ion beam mixing Ion implantation Multilayered Preferential sputtering Plasma source ion implantation Radiation-enhanced diffusion Radiation-induced segregation

Problems 10.1 Use the description of how a delta function distribution of particles spreads by diffusion to calculate the width of an initially sharply peaked distribution of: a) Vacancies b) Interstitials c) Self-tracer diffusing by vacancy mechanism. in Pt, after a time t = 1 min, for temperatures of 20 ◦C and 800 ◦C. 10.2 Consider a thin foil of a binary alloy in which the surface is the only defect sink. The foil is at thermal equilibrium at low temperature and is then heated instantaneously to near its melting point. Describe qualitatively the evolution of: a) The vacancy concentration b) The composition profile. 10.3 A bilayer of 50 nm Pd on top of 50 nm Ni is deposited on a silicon substrate. The layer is mixed with 300 keV Kr+ at a current of 40 μA/cm2 . Determine the sputtering yield. What is the maximum amount of Kr which can be implanted into this sample? 10.4 A Ni–1%Si alloy is heated to a temperature of 500 ◦C during irradiation by 500 keV Kr ions at a current density of 1μA/cm2 . a) What physical processes will be important in determining the surface concentration? b) If each process occurs independently of the others, what would be the effect of each on the surface composition? c) Estimate the combined effect of these processes on the surface composition and provide an argument to support your answer for the case where

Problems

541

i) Thermal processes dominate pure collisional processes ii) Pure collisional processes dominate thermal processes. Draw the composition vs. depth profile for cases (i) and (ii). B = 0.01 CSi B = 0.99 CNi

ΔHASi = −0.1 eV pSi /pNi = 2.0 ΔHmNi,v = 0.77 eV ΔHmNi,i = 0.1 eV ΔHmSi,v = 1.28 eV ΔHmSi,i = 0.15 eV RSι = 0.1176 nm RNi = 0.1245 nm CAsurface CAbulk −ΔHA = exp kT CBsurface CBbulk CAbulk CBbulk pA = surface pB CB CAsurface 10.5 A homogeneous A–B alloy of composition A–50 at%B is bombarded with 5 keV Ar ions at 400 ◦C. Given that the surface concentration following bombardment is 30% A and 70% B, describe what processes or combinations of processes could give rise to such behavior and which processes are dominant? v = migration enthalpy for A atoms by vacancies = 0.7 eV ΔHm,A v = migration enthalpy for B atoms by vacancies = 0.9 eV ΔHm,B i i ΔHm,A = ΔHm,B = migration enthalpy for A and B atoms via interstitials = 0.1 eV ΔHA = enthalpy of adsorption of A in B = −0.3 eV psA = sputtering probability for A atoms = 3 atoms/ion psB = sputtering probability for B atoms = 4 atoms/ion CA = constant × (dAv /dBv − dAi /dBi )Cv dAv α exp(−ΔHm,A /kT ) CAs /CBs = (CAb /CBb ) exp(−ΔHA /kT ) 10.6 Explain why ion beam mixing experiments often do not agree with the predictions from the ballistic theory of mixing. How would the temperature of the sample affect your answer?

542

10 Unique Effects of Ion Irradiation

10.7 A sample of polycrystalline Si is bombarded with 500 keV Al+ ions to a dose of 5 ×1015 i/cm2 . Given that Rp = 260 nm and ΔRp = 94 nm and that the damage profile has the same shape but peaks at 0.8Rp , calculate the peak damage in the material using reasonable assumptions. The distribution of ions is given by N(x) = Np exp(−X 2 ) where X = (x − Rp )/ΔRp , and Np = 0.4Ns /ΔRp. Assume that electronic stopping varies with energy as kE 1/2 where k = 1.5 × 10−16 eV1/2 cm2 . Energy transfer cross section based on inverse square law:

π 2 a2 Ea γ 1/2 8E 1/2 T 3/2 N = 3 ×1022 a/cm3 σ (E,T) =

Energy transfer cross section based on Rutherford scattering:

σ (E,T) =

π b20E γ 4T 2

Ec = 28 keV Ea = 14 keV Eb = 14 MeV Ed = 30 eV a = aB /(z1 z2 )1/6 aB = 0.053 nm b0 = z1 z2 ε 2 /η E ε 2 = 2aB ER 10.8 Explain the roles of cohesive energy and migration energy in ion beam mixing. What are the magnitudes of these energies and how can they influence ion beam mixing? Could a homogeneous alloy be unmixed? 10.9 A Cu–40%Ni target is irradiated with 100 keV Ar+ at a current density of 40 μA/cm2 . a) Determine which element will segregate to the surface under irradiation at 500 ◦C. b) On a single graph, draw the surface concentration as a function of time at 400 ◦C for the following processes: i) GA only ii) PS + RED iii) PS + RED + GA iv) PS + RED + RIS. GA = Gibbsian adsorption PS = Preferential sputtering RED = Radiation-enhanced diffusion RIS = Radiation-induced segregation Cu = 0.77 eV ΔHm,v Ni = 0.82 eV ΔHm,v Cu,Ni ΔHm,i = 0.12 eV

References

543

ΔHACu = −0.25 eV PCu = 5.5, PNi = 2.75 atoms/ion per unit concentration. 10.10 Determine the lateral load at which helium bubbles cause blistering in 316 stainless steel under the condition that the blister diameter ∼tB2 , where tB is the blister cap thickness.

References 1. Nastasi M, Mayer JW, Hirvonen JK (1996) Ion-Solid Interactions: Fundamentals and Applications. Cambridge University Press, Cambridge 2. Komarov F (1992) Ion Beam Modification of Materials. Gordon and Breach, Philadelphia 3. Was GS (1989) Prog Surf Sci 32(3/4):211–312 4. Smidt F (1990) Int Mater Rev 35(2):61–128 5. Hirvonen JK (1991) Mater Sci Rep 6:251–274 6. Sigmund P (1969) Phys Rev 184:383 7. Smith DL (1978) J Nucl Mater 75:20–31 8. Sigmund P (1981) In: Sputtering by Particle Bombardment I. Springer, Berlin Heidelberg New York, p 9 9. Winters HF (1976) In: Kaminsky M (ed) Radiation Effects in Solid Surfaces. American Chemical Society, Washington, DC, p 1 10. Lindhard J, Nielsen V, Scharff M (1968) Kgl Danske Videnskab Selskab Mat Fys Medd 36(10):1 11. Wiedersich H, Andersen HH, Lam NQ, Rehn LE, Pickering HW (1983) In: Poate JM, Foti G, Jacobson DC (eds) Surface Modification and Alloying, NATO Series on Materials Science. Plenum, New York, p 261 12. Falcone G, Sigmund P (1981) Appl Phys 25:307 13. Lam NQ, Wiedersich H (1987) Nucl Instr Meth B 18:471 14. Wynblatt P, Ku RC (1979) In: Johnson WC, Blakely JM (eds) Interfacial Segregation. American Society for Metals, Metals Park, OH, p 115 15. Sigmund P (1979) J Appl Phys 50(11):7261 16. Sigmund P, Gras-Marti A (1981) Nucl Instr Meth 182/183:25 17. Gras-Marti A, Sigmund P (1981) Nucl Instr Meth 180:211 18. Myers SM (1980) Nucl Instr Meth 168:265 19. Anderson HH (1979) Appl Phys (Germany) 18:131 20. Workman TW, Cheng YT, Johnson WL, Nicolet MA (1987) Appl Phys Lett 50(21):1485 21. Westendorp H, Wang ZL, Saris FW (1982) Nucl Instr Meth 194:453 22. Wang ZL, Westendorp JFM, Doorn S, Saris FW (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier, New York, p 59 23. Paine BM, Averback RS (1985) Nucl Instr Meth B 7/8:666 24. Johnson WL, Cheng Y-T, Van Rossum M, Nicolet M-A (1985) Nucl Instr Meth B 7/8:657 25. Van Rossum M, Cheng Y-T (1988) Defect Diffusion Forum 57/58:1 26. Cheng Y-T, Workman TW, Nicolet M-A, Johnson WL (1987) In: Beam-Solid Interactions and Transient Processes, vol 74. Materials Research Society, Pittsburgh, PA, p 419 27. Ma E, Workman TW, Johnson WL, Nicolet M-A (1989) Appl Phys Lett 54(5):413 28. Cheng Y-T, Van Rossum M, Nicolet M-A, Johnson WL (1984) Appl Phys Lett 45(2):185 29. Van Rossum M, Cheng Y-T, Nicolet M-A, Johnson WL (1985) Appl Phys Lett 46(6):610

544 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41.

42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57.

10 Unique Effects of Ion Irradiation Rossi F, Nastasi M (1991) J Appl Phys 69(3):1310 Vineyard GH (1976) Rad Eff 29:245 Matteson S, Roth J, Nicolet M, Rad Eff 42 (1979) 217–226 Cheng Y-T (1989) Phys Rev B 40(10):7403–7405 Hung LS, Mayer JW (1985) Nucl Instr Meth B 7/8:676 Was GS, Eridon JM (1987) Nucl Instr Meth B 24/25:557 Lam NQ, Leaf GK, Wiedersich H (1980) J Nucl Mater 88:289 Lam NQ, Wiedersich H (1982) In: Picraux ST, Choyke WJ (eds) Metastable Materials Formation by Ion Implantation. Elsevier, New York, p 35 Lam NQ, Wiedersich H (1981) J Nucl Mater 103/104:433 Lam NQ, Leaf GK (1986) J Mater Res 1:251 Rehn LE, Okamoto PR (1983) In: Nolfi FV (ed) Phase Transformations During Irradiation. Applied Science, New York, p 247 Mayer SGB, Milillo FF, Potter DI (1985) In: Koch CC, Liu CT, Stoloff NS (eds) HighTemperature Ordered Intermetallic Alloys, vol 39. Materials Research Society, Pittsburgh, PA, p 521 Liu JC, Mayer JW (1987) Nucl Instr Meth B 19/29:538 Alexander D, Was G, Rehn LE (1990) Materials Research Symposium, vol 157. Materials Research Society, Pittsburgh, PA, p 155 Eridon J, Rehn L, Was GS (1987) Nucl Instr Meth B 19/20:626 Ahmed M, Potter DI (1987) Acta Metal 35(9):2341 Nishiyama Z (1978) In: Fine ME, Meshii M, Wayman CM (eds) Martensitic Transformations, vol 7. Academic, New York Bradley RM, Harper JME, Smith DA (1986) J Appl Phys 60:4160 Ma Z, Was GS (1999) J Mater Res 14(10):4051–4061 Didenko AN, Kozlov EV, Sharkeev YuN, Tailashev AS, Rajabchikov AI, Pranjavichus L, Augulis L (1993) Surf Coat Technol 56:97–104 Behrisch R, Risch M, Roth J, Scherzer BMU (1976) Proceedings of the 9th Symposium on Fusion Technology. Pergamon, New York, pp 531–539 Ullmaier H (1983) Rad Eff 78:1–10 Wolfer WG (1980) J Nucl Mater 93/94:713–720 Behrisch R, Scherzer BMU (1983) Rad Eff 78:393–403 Birtcher RC, J¨ager W (1987) Ultramicroscopy 22:267–280 Liu AS, Birtcher RC (1989) Mat Res Soc Symp, vol 128. Materials Research Society, Pittsburgh, PA, pp 303–308 Johnson PR (1983) Rad Eff 78:147–156 Mazey DJ, Evans JH (1986) J Nucl Mater 138:16–18

11 Simulation of Neutron Irradiation Effects with Ions

Radiation effects research is conducted with a variety of energetic particles: neutrons, electrons, light ions and heavy ions. Energetic ions can be used to understand the effects of neutron irradiation in reactor components, and interest in this application of ion irradiation has grown in recent years for several reasons that include the avoidance of high residual radioactivity and the decline of neutron sources for materials irradiation. The damage state and microstructure resulting from ion irradiation, and thus the degree to which ion irradiation emulates neutron irradiation, depend upon the particle type and the damage rate. This chapter will begin with a brief review of the damage function, primary recoil spectrum and efficiency of defect production for various particle types. Effects of particle type on both microstructure and microchemistry will be discussed, followed by the effects of the irradiated microstructure on mechanical properties. The roles of dose, dose rate, and temperature parameters and the constraints on parameter space by each particle source will be discussed and compared against the effects of neutron irradiation.

11.1 Motivation for Using Ion Irradiation as a Surrogate for Neutron Irradiation In the 1960s and 1970s, heavy ion irradiation was developed for the purpose of simulating neutron damage in support of the fast breeder reactor program [1, 2, 3]. Ion irradiation and simultaneous He injection have also been used to simulate the effects of 14 MeV neutron damage in conjunction with the fusion reactor engineering program. The application of ion irradiation (defined here as any charged particle, including electrons) to the study of neutron irradiation damage is of interest to the light water reactor community to address issues such as stress corrosion cracking of core materials that are affected by irradiation [4, 5, 6]. Ion irradiation is also being used to understand the irradiated microstructure of reactor pressure vessel steels, Zircaloy fuel cladding, and materials for advanced reactor concepts. There is significant incentive to use ion irradiation to study neutron damage as this technique has the potential for yielding answers on basic processes in addition to the potential for enormous savings in time and money. Neutron irradiation experiments are not amenable to studies involving a wide range of conditions, which is precisely what is required for investigations of the basic damage processes. Radi-

546

11 Simulation of Neutron Irradiation Effects with Ions

ation damage simulation by ions allows easy variation of the irradiation parameters such as dose, dose rate and temperature over a wide range of values. Typical neutron irradiation experiments in test reactors require 1–3 years of incore exposure to reach appreciable fluence levels for accelerated post-irradiation testing. However, this is accompanied by at least another year of capsule design and preparation as well as disassembly and cooling. Analysis of microchemical changes by Auger electron spectroscopy (AES) or microstructural changes by energy dispersive spectroscopy via scanning transmission electron microscopy (STEM-EDS) and mechanical property or stress corrosion cracking (SCC) evaluation can take several additional years because of the precautions, special facilities and instrumentation required for handling radioactive samples. The result is that a single cycle from irradiation through microanalysis and mechanical property/SCC testing may take between three and five years. Such a long cycle length does not permit for iteration on irradiation or material conditions that is critical in any experimental research program. The long lead time required for design and irradiation also reduces flexibility in altering irradiation programs as new data becomes available. Because of the long cycle time, the requirement of special facilities and special sample handling, the costs for neutron irradiation experiments are very high. In contrast to neutron irradiation, ion (heavy, light or electrons) irradiation enjoys considerable advantages in both cycle length and cost. Ion irradiations of any type rarely require more than several tens of hours to reach damage levels in the 1–10 dpa range. Ion irradiation produces little or no residual radioactivity, allowing handling of samples without the need for special precautions. These features translate into significantly reduced cycle length and cost. The challenge is then to verify the equivalency of the results of neutron and ion irradiation. The key question that needs to be answered is how do results from neutron and charged particle irradiation experiments compare? How, for example is one to compare the results of a component irradiated in-core at 288 ◦C to a fluence of 1 ×1021 n/cm2 (E > 1 MeV) over a period of 8.5 months, with an ion irradiation experiment using 3 MeV protons at 400 ◦C to 1 dpa (displacements per atom) at a dose rate of 10−5 dpa/s (∼1 day), or 5 MeV Ni++ at 500 ◦C to 10 dpa at a dose rate of 5 ×10−3 dpa/s (∼1 hr)? The first question to resolve is the measure of radiation effect. In the irradiation assisted stress corrision cracking (IASCC) problem in LWRs, concern has centered on two effects of irradiation: segregation of major alloying elements or impurities to grain boundaries, which then cause embrittlement or enhance the intergranular stress corrosion cracking (IGSCC) process, and hardening of the matrix that results in localized deformation and embrittlement. The appropriate measure of the radiation effect in the former case would then be the alloy concentration at the grain boundary or the amount of impurity segregated to the grain boundary. This quantity is measurable by analytical techniques such as AES or STEM-EDS. For the latter case, the measure of the radiation effect would be the nature, size, density and distribution of dislocation loops, black dots and the total dislocation network, and how they impact the deformation of the alloy. Hence, spe-

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation

547

cific and measurable effects of irradiation can be determined for both neutron and ion irradiation experiments. The next concern is determining how ion irradiation translates into the environment describing neutron irradiation. That is, what are the irradiation conditions required for ion irradiation to yield the same measure of radiation effect as that for neutron irradiation? This is the key question, for in a post-irradiation test program, it is only the final state of the material that is important in the determination of equivalence, and not the path taken. Therefore, if one could devise ion irradiation experiments that yielded the same measures of irradiation effects as observed in neutron irradiation experiments, then the data obtained in post-irradiation experiments will be equivalent. In such a case, ion irradiation experiments can provide a direct substitute for neutron irradiation. While neutron irradiation will always be required to qualify materials for reactor application, ion irradiation provides a low cost and rapid means of elucidating mechanisms and screening materials for the most important variables.

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation The first problem in determining the equivalence between the measure of radiation effect in charged particle and neutron irradiation is the use of a common dose unit. Recall from the introduction that irradiated materials properties can be more successfully compared using dpa as a measure of exposure. The basic (measurable) dose unit for neutron irradiation is the fluence in (n/cm2) above some energy threshold (E > x MeV), where x is the energy threshold. For charged particles it is the integrated current or charge in units of Q/cm2 . Both of these measures can be converted to dose in units of dpa and dose rate as dpa/s using one of several models for the determination of dpa, as shown in Chap. 2. A fundamental difference between ion and neutron irradiation effects is the particle energy spectrum that arises due to the difference in how the particles are produced. Ions are produced in accelerators and emerge in monoenergetic beams with vary narrow energy widths. However, the neutron energy spectrum in a reactor extends over several orders of magnitude in energy, thus presenting a much more complicated source term for radiation damage. Figure 11.1 shows the considerable difference in neutron and ion energy spectra and also between neutron spectra in different reactors and at different locations within the reactor vessel. Another major difference in the characteristics of ions and neutrons is their depth of penetration. As shown in Fig. 2.25 of Chap. 2, ions lose energy quickly because of high electronic energy loss, giving rise to a spatially non-uniform energy deposition profile caused by the varying importance of electronic and nuclear energy loss during the slowing down process. Their penetration distances range between 0.1 and 100 μm for ion energies that can practically be achieved by laboratory-scale accelerators or implanters. By virtue of their electrical neutrality, neutrons can penetrate

548

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.1. Energy spectra of incident ions in a monoenergetic ion beam, and neutrons from a variety of reactor types (from [7])

very large distances and produce spatially flat damage profiles over many millimeters of material. As discussed in Chap. 2, the total number of displacements per atom is given by the K–P [8] or NRT [9] models. This quantity provides an adequate measure of the number of displacements created by the incoming particle irrespective of the mass of the particle. In addition to dpa, the primary recoil spectrum describes the relative number of collisions in which an energy between T and T + dT is transferred from the primary recoil atom to other target atoms. The fraction of recoils between the displacement energy Ed , and T is, from Eq. (3.11): 1 P(Ei , T ) = N

T Ed

σ (Ei , T ) dT

(11.1)

where N is the total number of primary recoils and σ (Ei , T ) is the differential cross section for a particle of energy Ei to create a recoil of energy T , and Ed is the displacement energy. The recoil fraction is shown in Fig. 3.5, which reveals only a small difference between ions of very different masses. But there is a substantial difference in the damage morphology between particles of different mass. Light ions such as electrons and protons will produce damage as isolated Frenkel pairs or in small clusters while heavy ions and neutrons produce

11.2 Review of Aspects of Radiation Damage Relevant to Ion Irradiation

549

damage in large clusters (see Fig. 3.7). For 1 MeV particle irradiation of copper, half the recoils for protons are produced with energies less than ∼60 eV while the same number for Kr occurs at about 150 eV. Recoils are weighted toward lower energies because of the screened Coulomb potential that controls the interactions of charged particles. For an unscreened Coulomb interaction, the probability of creating a recoil of energy T varies as 1/T 2 . However, neutrons interact as hard spheres and the probability of a creating a recoil of energy T is independent of recoil energy. In fact, a more important parameter describing the distribution of damage over the energy range is a combination of the fraction of defects of a particular energy and the damage energy. Described in Chap. 3, the weighted average recoil spectrum, W (Ei , T ) weights the primary recoil spectrum by the number of defects or the damage energy produced in each recoil: W (Ei , T ) =

ED (Ei ) =

1 ED (Ei )

Tˆ Ed

T Ed

σ (Ei , T )ED (T ) dT ,

σ (Ei , T )ED (T ) dT ,

(11.2)

(11.3)

where Tˆ is the maximum recoil energy given by Tˆ = Ei = 4Ei M1 M2 /(M1 + M2 )2 . As described in Chap. 3, for the extremes of Coulomb and hard-sphere interactions, the weighted average recoil spectra for each type of interaction is: WCoul (Ei , T ) = WHS (Ei , T ) =

ln T − ln Ed ln Tˆ − ln Ed

T 2 − Ed2 . Ed2

(11.4a)

(11.4b)

Equations (11.4a) and (11.4b) are graphed in Fig. 3.6 for 1 MeV particle irradiations of copper. The Coulomb forces extend to infinity and slowly increase as the particle approaches the target, hence the slow increase with energy. In a hard-sphere interaction, the particles and target do not feel each other until their separation reaches the hard-sphere radius at which point the repulsive force goes to infinity. A screened Coulomb potential is most appropriate for heavy ion irradiation. Note the large difference in W (Ei , T ) between the various types of irradiations. While heavy ions come closer to reproducing the energy distribution of recoils of neutrons than do light ions, neither is accurate in the tails of the distribution. This does not mean that ions are poor simulations of radiation damage, but it does mean that damage is produced differently and this difference will need to be considered when designing an irradiation program that is intended to produce microchemical and microstructural changes that match those from neutron irradiation. The actual number of defects that survive the displacement cascade and their spatial distribution in the solid will determine the effect on the irradiated microstructure. This topic was covered in Chaps. 3 and 7 by classification of defects according

550

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.2. History of point defects after creation in the displacement cascade

to their behavior in the solid. Figure 11.2 summarizes the effect of damage morphology from the viewpoint of the grain boundary and how the defect flow affects radiation-induced grain boundary segregation. Despite the equivalence in energy among the four particle types described in Fig. 3.7, the average energy transferred and the defect production efficiencies vary by almost two orders of magnitude! This is explained by the differences in the cascade morphology among the different particle types. Neutrons and heavy ions produce dense cascades that result in substantial recombination during the cooling or quenching phase. However, electrons are just capable of producing a few widely spaced Frenkel pairs that have a low probability of recombination. Protons produce small widely spaced cascades and many isolated FPs due to the Coulomb interaction and therefore, fall between the extremes in displacement efficiency defined by electrons and neutrons.

11.3 Particle Type Dependence of RIS We will focus on the comparison between four types of particle irradiation in order to outline a methodology for establishing equivalence between neutron and charged particle irradiation. We will further focus on radiation-induced segregation as the

11.3 Particle Type Dependence of RIS

551

measure of the effect of irradiation in order to compare the particles. RIS is selected because it depends only on the action of point defects, and not on their agglomeration. The irradiation parameters for the four particle types are given in Table 11.1. Each experiment is characterized by the particle type, energy and irradiation temperature, reported dose rate and reported total dose. The last column is the dose to reach a steady state RIS profile using the Perk’s model [11]. The columns labeled reported and corrected refer to RIS calculations using the nominal dose rate (reported value) and the efficiency-corrected (corrected value), respectively. The displacement efficiency is calculated using Naundorf’s model, described in Chap. 3. A quantity of interest in RIS for LWR core materials is the amount of chromium depleted from the grain boundary, or the area inside the Cr concentration profile (Fig. 11.3). In other reactor systems, other elements may be of interest due to the potential for in-reactor precipitation. The appropriate measure of depletion is somewhat questionable. One could use the grain boundary chromium value as the measure of the extent of chromium depletion. Alternatively, the FWHM of the depletion profile has been used. In fact both of these quantities are useful and can be obtained from measured depletion profiles. However, the area inside the Cr concentration profile represents changes to a volume of material and is more sensitive to changes in the profile shape than either the grain boundary value or the FWHM alone. The amount of Cr depletion is determined by integrating the concentration profile for

Fig. 11.3. Definition of the segregated area, M in a quantitative assessment of RIS

552

11 Simulation of Neutron Irradiation Effects with Ions

Table 11.1. Comparison of irradiation parameters and RIS for different particle types (from [10]) Particle type

Energy Temp Effic. (MeV) (◦C)

Electrons

1.0

450

Dose rate (dpa/s) rept’d corr’d∗

1.0

2 ×10−3 2 ×10−3

Protons

3.4

360

0.2

7×10−6

Ni ions

5.0

500

0.04

5×10−3 2×10−4

Neutrons Fission 288 reactor ∗ ∗∗

0.02

∼5 × 0−8

Total dose Dose to (dpa) steady state∗∗ (dpa) rept’d corr’d rept’d corr’d 10

10

28

28

0.2

7

3

0.4

25

7

1×10−6

1 10 1

0.02

4

9×10−10

1.4

Efficiency corrected value As calculated by the Perks model [11] for RIS

that element with distance from the grain boundary: l(t) CA0 − CA (x,t) dx , M=

(11.5)

0

where M is the segregated area, CA0 is the bulk atom concentration, CA (x,t) is the atom concentration near the surface, and l(t) is the half width of the depleted zone. Figures 11.4a,b show the amount of grain boundary chromium depletion as a function of irradiation dose (Fig. 11.4a) and time (Fig. 11.4b) for each of the four particles described in Table 11.1. The calculated values of Cr depletion for each of the particle types using reported and corrected dose rates, according to the freely migrating defect production efficiencies, are shown by the open and closed symbols, respectively. Since electrons are assumed to be 100% efficient in producing defects available to affect segregation, there is no change in the segregated area after accounting for efficiency. However, there is a difference with protons, heavy ions and neutrons, which amounts to a reduction in the amount of segregation. The difference is largest for neutrons and smallest for protons. The difference is a function of not only the displacement efficiency, but also the slope of the dose rate curves. Nevertheless, substantial differences result in the expected amounts of grain boundary segregation when the displacement efficiency is taken into account. Figure 11.5a shows the calculated amount of Cr depletion as a function of temperature for several displacement rates at steady state. Steady state is reached at different dose levels for each experiment. At a given displacement rate, the segregated area peaks at some intermediate temperature and falls off at both higher and lower temperatures. This is due to the dominance of recombination at low temperatures and back diffusion at high temperatures [10]. Also note that the effect of a decreasing displacement rate is to shift the curves to higher maxima at lower temperatures. For a given dose, a lower displacement rate yields lower steady state defect concentrations, reducing the number of defects lost to recombination, and shifting the curve to lower temperatures while increasing the degree of segregation. Figure 11.5a also shows the effect of three of the four parameters defining an experiment:

11.3 Particle Type Dependence of RIS

553

Fig. 11.4. Chromium depletion vs. (a) dose and (b) irradiation time, for several particle types, and the effect of correcting for particle efficiency (from [10])

554

11 Simulation of Neutron Irradiation Effects with Ions

particle type, temperature and dose rate. It does not show the effect of dose since this is a steady state result that is achieved at different doses for each of the experiments described in Table 11.1. Figure 11.5b shows the dose required to reach steady state as a function of temperature and dose rate. Each of the experiments is plotted for both the reported and the corrected displacement rates. Note the large difference in the dose to reach steady state between electrons and neutrons. In general, irradiation at a lower dpa rate will result in a lower dose to reach steady state and the difference is greatest for this comparison. Correspondingly, proton and heavy ion irradiation fall between neutrons and electrons for the experiments described in Table 11.1. This can be understood by considering the chemical rate equations given in Eq. (5.1), where the first term is the production rate, the second is the loss by mutual recombination and 1/2 the third is the loss by annihilation of defects at sinks. At steady state, Ci,v α K0 at low temperature and Ci,v α K0 at high temperature (see Chap. 5). So the resulting point defect concentrations are strong functions of the production rate. Figure 11.6 shows a plot of segregation as a function of temperature for particles with displacement rates characteristic of their sources. Note that the temperature at which segregation is a maximum (concentration is a minimum) shifts to higher values with increasing dose rate. This is due to the trade-off between temperature and dose rate. The temperature-dose rate interdependence for stainless steel over a wide range of temperatures and dose rates is shown in Fig. 11.7. Also noted are the regions in which reactor irradiation by neutrons, and where proton and Ni ion irradiations occur. This graph explains why the experiments conducted at the highest dose rates are also conducted at the highest temperatures. A simple method for examining the trade-off between dose rate and temperature in comparing irradiation effects from different particle types is found in the invariance requirements discussed in Chap. 8. For a given change in dose rate, we would like to know what change in temperature (at the same dose) is required to cause the same number of defects to be absorbed at sinks. The number of defects per unit volume that are lost to sinks up to time τ is: NSj =

τ

2 kSj Cj dt ,

(11.6)

0

and the ratio of ratio of vacancy loss to interstitial loss is: RS =

NSv , NSi

(11.7)

where j = v or i, and kS2 is the sink strength. The quantity NS is important in describing microstructure development involving total point defect flux to sinks (e.g., RIS). The number of defects per unit volume that have recombined up to time τ is given by: NR = Kiv

τ 0

CiCv dt ,

(11.8)

11.3 Particle Type Dependence of RIS

555

Fig. 11.5. (a) Chromium depletion, and (b) dose to reach steady state, as functions of temperature, dose rate and particle efficiency (from [10])

556

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.6. Dependence of grain boundary chromium concentration on temperature for particles with various dose rates and defect generation efficiencies (from [10])

where Kiv is the vacancy–interstitial recombination coefficient. NR is the relevant quantity for the growth of defect aggregates such as voids and loops that require partitioning of point defects to allow growth. The invariance requirements can be used to prescribe an ion irradiation temperature-dose rate combination that simulates neutron radiation. We take the example of irradiation of stainless steel under typical boiling water reactor (BWR) core irradiation conditions of ∼4.5 ×10−8 dpa/s at 288 ◦C. If we were to conduct a proton irradiation with a characteristic dose rate of 7.0 ×10−6 dpa/s, then using Eq. (8.158) with a vacancy formation energy of 1.9 eV and a vacancy migration energy of 1.3 eV, the experiment will be invariant in NS with the BWR core irradiation (e.g., RIS), for a proton irradiation at 400 ◦C. Similarly, using Eq. (8.162), an irradiation temperature of 300 ◦C will result in an invariant NR (e.g., swelling or loop growth). For a Ni++ ion irradiation at a dose rate of 10−3 dpa/s, the respective temperatures are 675 ◦C (NS invariant) and 340 ◦C (NR invariant). In other words, the temperature “shift” due to the higher dose rate is dependent on the microstructure feature of interest. Also, with increasing difference in dose rate, the ΔT between proton and ion irradiation increases substantially. The nominal irradiation temperatures selected for proton irradiation, 360 ◦C and for Ni++ irradiation, 500 ◦C represent compromises between the extremes for invariant Ns and NR .

11.4 Advantages and Disadvantages of the Various Particle Types

557

Fig. 11.7. Relation between temperature and dose rate in the context of radiation-induced segregation, and the locations of neutron, proton and nickel ion irradiations

11.4 Advantages and Disadvantages of the Various Particle Types Each particle type has its advantages and disadvantages for use in the study or emulation of radiation effects. Common disadvantages of charged particle beams are the lack of transmutation reactions and the need to use a raster-scanned beam. With the exception of some minor transmutation reactions that can occur with light ion irradiation, charged particles do not reproduce the types of transmutation reactions that occur in reactor core materials due to interaction with neutrons. The most important of these is the production of He by transmutation of Ni or B. But a second consideration is that of a raster-scanned beam in which any volume element of the target is exposed to the beam for only a fraction of the raster-scan cycle. For a typical beam scanner and beam parameters, the fraction of time that any particular volume element in the solid is being bombarded is ∼0.025. Thus, the instantaneous dose rate during the beam-on portion of the cycle is 40 times that of the average (Fig. 11.8). The result is that the defect production rate is very high and defects can anneal out in the remaining 0.975 portion of the cycle before the beam again passes through the volume element. As such, the effective defect production rate in raster-scanned systems will be less, and must be accounted for. While one objective of ion irradiation is to emulate the effect of neutrons, a second is to understand basic physical radiation damage processes, for which neutron

558

11 Simulation of Neutron Irradiation Effects with Ions

Fig. 11.8. The effect of a raster-scanned beam on the instantaneous production rate of point defects with the same time averaged rate as a continuous source (from [12])

irradiation is often less well-suited. While ion irradiation can be conducted with great control over temperature, dose rate and total dose, such control is a challenge to reactor irradiations. For example, instrumented tubes with active temperature control are expensive to design, build and operate. Even so, frequent power changes can be difficult to handle as the flux-temperature relationship will change and this can result in artifacts in the irradiated microstructure (see Sect. 8.3.11 and Fig. 8.51). On the other hand, cheaper “rabbit” tube irradiations use passive gamma heating and temperatures are not known with any certainty. Similarly, doses and dose rates are most often determined by neutronic models of the core locations and are not verifiable. As such, ion irradiations enjoy the advantage of better control and verification of irradiation conditions as compared to neutron irradiation. Table 11.2 provides a list of advantages and disadvantages for each of three particle types; electrons, heavy ions and light ions (protons), and they are discussed in detail in the following sections. 11.4.1 Electrons Electron irradiation is easily conducted in a high voltage transmission electron microscope and as such, it uses a rather simple ion source, that being either a hot filament or a field emission gun. An advantage is that the same instrument used for irradiation damage can be used to image the damage. Another advantage is that the

11.4 Advantages and Disadvantages of the Various Particle Types

559

Table 11.2. Advantages and disadvantages of irradiations with various particle types (from [12]) Electrons Advantages Disadvantages Relatively “simple” source – TEM Energy limited to ∼1 MeV Uses standard TEM sample no cascades High dose rate – short irradiation times Very high beam current (high dpa rate) requires high temperature Poor control of sample temperature Strong “Gaussian” shape (nonuniform intensity profile) to beam No transmutation Heavy Ions Advantages Disadvantages High dose rate – short irradiation times Very limited depth of penetration Strongly peaked damage profile High Tavg Cascade production Very high beam current (high dpa rate) requires high temperature No transmutation Potential for composition changes at high dose via implanted ion Advantages Accelerated dose rate – moderate irradiation times Modest ΔT required Good depth of penetration Flat damage profile over tens of μ m

Protons Disadvantages Minor sample activation Smaller, widely separated cascades No transmutation

high dose rate requires very short irradiation time, but this will also require a large temperature shift as explained in the previous section. There are several disadvantages to electron irradiation using a TEM. First, energies are generally limited to 1 MeV. This energy is sufficient to produce an isolated Frenkel pair in transition metals, but not cascades. The high dose rate requires high temperatures that must be closely monitored and controlled, which is difficult to do precisely in a typical TEM sample stage. Another drawback is that since irradiations are often conducted on thin foils, defects are created in close proximity to the surface and their behavior may be affected by the presence of the surface. Perhaps the most serious drawback is the Gaussian shape to the electron beam that can give rise to strong dose rate gradients across the irradiated region. Figure 11.9 shows the composition profile of copper around a grain boundary in Ni–39%Cu following electron irradiation. Note that while there is local depletion at the grain boundary (as expecte